Continuum Mechanics and Plasticity
© 2005 by Chapman & Hall/CRC Press
CRC S ERIES: M ODERN M ECHANICS
AND
M ATHEMAT...

Author:
Han-Chin Wu

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Continuum Mechanics and Plasticity

© 2005 by Chapman & Hall/CRC Press

CRC S ERIES: M ODERN M ECHANICS

AND

M ATHEMATICS

Series Editors: David Gao and Ray W. Ogden

PUBLISH E D TITLE S

BEYOND PERTURBATION: INTRODUCTION

TO THE

HOMOTOPY ANALYSIS METHOD

by Shijun Liao

MECHANICS OF ELASTIC COMPOSITES by Nicolaie Dan Cristescu, Eduard-Marius Craciun, and Eugen Soós

CONTINUUM MECHANICS

AND PLASTICITY

by Han-Chin Wu

FO RTH CO MIN G TITLE S

HYBRID INCOMPATIBLE FINITE ELEMENT METHODS by Theodore H.H. Pian, Chang-Chun Wu

MICROSTRUCTURAL RANDOMNESS by Martin Ostroja Starzewski

© 2005 by Chapman & Hall/CRC Press

IN

MECHANICS

OF

MATERIALS

Continuum Mechanics and Plasticity

Han-Chin Wu

CHAPMAN & HALL/CRC A CRC Press Company Boca Raton London New York Washington, D.C.

© 2005 by Chapman & Hall/CRC Press

Library of Congress Cataloging-in-Publication Data Wu, Han-Chin. Continuum mechanics and plasticity / Han-Chin Wu. p. cm. — (Modern mechanics and mathematics series ; no. 3) Includes index. ISBN 1-58488-363-4 (alk. paper) 1. Continuum mechanics. 2. Plasticity. I. Title. II. CRC series—modern mechanics and mathematics ; 3. QA808.2.W8 2004 531—dc22

2004055118

This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. A wide variety of references are listed. Reasonable efforts have been made to publish reliable data and information, but the author and the publisher cannot assume responsibility for the validity of all materials or for the consequences of their use. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming, and recording, or by any information storage or retrieval system, without prior permission in writing from the publisher. The consent of CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from CRC Press for such copying. Direct all inquiries to CRC Press, 2000 N.W. Corporate Blvd., Boca Raton, Florida 33431. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe.

Visit the CRC Press Web site at www.crcpress.com © 2005 by Chapman & Hall/CRC Press No claim to original U.S. Government works International Standard Book Number 1-58488-363-4 Library of Congress Card Number 2004055118 Printed in the United States of America 1 2 3 4 5 6 7 8 9 0 Printed on acid-free paper

© 2005 by Chapman & Hall/CRC Press

Contents

Preface

xiii

Author

xvii

Part I

Fundamentals of Continuum Mechanics

1

Cartesian Tensors 1.1 Introduction 1.1.1 Notations 1.1.2 Cartesian Coordinate System 1.1.3 Special Tensors 1.2 Vectors 1.2.1 Base Vectors and Components 1.2.2 Vector Addition and Multiplication 1.2.3 The e–δ Identity 1.3 The Transformation of Axes 1.4 The Dyadic Product (The Tensor Product) 1.5 Cartesian Tensors 1.5.1 General Properties 1.5.2 Multiplication of Tensors 1.5.3 The Component Form and Matrices 1.5.4 Quotient Law 1.6 Rotation of a Tensor 1.6.1 Orthogonal Tensor 1.6.2 Component Form of Rotation of a Tensor 1.6.3 Some Remarks 1.7 The Isotropic Tensors 1.8 Vector and Tensor Calculus 1.8.1 Tensor Field 1.8.2 Gradient, Divergence, Curl 1.8.3 The Theorem of Gauss References Problems

3 3 3 4 4 5 5 5 6 8 12 13 13 16 18 19 20 20 22 23 28 34 34 34 37 40 41

2

Stress 2.1 Introduction 2.2 Forces

45 45 45 v

© 2005 by Chapman & Hall/CRC Press

vi

Contents 2.3 2.4 2.5 2.6 2.7 2.8 2.9

Stress Vector The Stress Tensor Equations of Equilibrium Symmetry of the Stress Tensor Principal Stresses Properties of Eigenvalues and Eigenvectors Normal and Shear Components 2.9.1 Directions Along which Normal Components of σij Are Maximized or Minimized 2.9.2 The Maximum Shear Stress 2.10 Mean and Deviatoric Stresses 2.11 Octahedral Shearing Stress 2.12 The Stress Invariants 2.13 Spectral Decomposition of a Symmetric Tensor of Rank Two 2.14 Powers of a Tensor 2.15 Cayley–Hamilton Theorem References Problems

3

Motion and Deformation 3.1 Introduction 3.2 Material and Spatial Descriptions 3.2.1 Material Description 3.2.2 Spatial Description 3.3 Description of Deformation 3.4 Deformation of a Neighborhood 3.4.1 Homogeneous Deformations 3.4.2 Nonhomogeneous Deformations 3.5 The Deformation Gradient 3.5.1 The Polar Decomposition Theorem 3.5.2 Polar Decompositions of the Deformation Gradient 3.6 The Right Cauchy–Green Deformation Tensor 3.6.1 The Physical Meaning 3.6.2 Transformation Properties of CRS 3.6.3 Eigenvalues and Eigenvectors of CRS 3.6.4 Principal Invariants of CRS 3.7 Deformation of Volume and Area of a Material Element 3.8 The Left Cauchy–Green Deformation Tensor 3.9 The Lagrangian and Eulerian Strain Tensors 3.9.1 Deﬁnitions 3.9.2 Geometric Interpretation of the Strain Components 3.9.3 The Volumetric Strain 3.10 Other Strain Measures 3.11 Material Rate of Change 3.11.1 Material Description of the Material Derivative 3.11.2 Spatial Description of the Material Derivative

© 2005 by Chapman & Hall/CRC Press

46 47 50 52 53 55 59 60 60 64 65 66 69 71 72 73 74 79 79 80 80 81 83 83 85 86 88 88 90 98 98 101 103 104 105 108 108 108 112 115 118 119 119 120

Contents

4

3.12 Dual Vectors and Dual Tensors 3.13 Velocity of a Particle Relative to a Neighboring Particle 3.14 Physical Signiﬁcance of the Rate of Deformation Tensor 3.15 Physical Signiﬁcance of the Spin Tensor 3.16 Expressions for D and W in Terms of F 3.17 Material Derivative of Strain Measures 3.18 Material Derivative of Area and Volume Elements References Problems

122 124 125 128 129 131 132 133 134

Conservation Laws and Constitutive Equation 4.1 Introduction 4.2 Bulk Material Rate of Change 4.3 Conservation Laws 4.3.1 The Conservation of Mass 4.3.2 The Conservation of Momentum 4.3.3 The Conservation of Energy 4.4 The Constitutive Laws in the Material Description 4.4.1 The Conservation of Mass 4.4.2 The Conservation of Momentum 4.4.3 The Conservation of Energy 4.5 Objective Tensors 4.6 Property of Deformation and Motion Tensors Under Reference Frame Transformation 4.7 Objective Rates 4.7.1 Some Objective Rates 4.7.2 Physical Meaning of the Jaumann Stress Rate 4.8 Finite Elasticity 4.8.1 The Cauchy Elasticity 4.8.2 Hyperelasticity 4.8.3 Isotropic Hyperelastic Materials 4.8.4 Applications of Isotropic Hyperelasticity 4.9 Inﬁnitesimal Theory of Elasticity 4.9.1 Constitutive Equation 4.9.2 Homogeneous Deformations 4.9.3 Boundary-Value Problems 4.10 Hypoelasticity References Problems

141 141 142 145 145 146 148

Part II 5

vii

150 150 151 163 164 166 169 169 172 174 175 177 181 185 193 193 195 197 197 200 200

Continuum Theory of Plasticity

Fundamentals of Continuum Plasticity 5.1 Introduction

© 2005 by Chapman & Hall/CRC Press

205 205

viii

6

7

Contents 5.2

Some Basic Mechanical Tests 5.2.1 The Uniaxial Tension Test 5.2.2 The Uniaxial Compression Test 5.2.3 The Torsion Test 5.2.4 Strain Rate, Temperature, and Creep 5.3 Modeling the Stress–Strain Curve 5.4 The Effects of Hydrostatic Pressure 5.5 Torsion Test in the Large Strain Range 5.5.1 Introduction 5.5.2 Experimental Program and Procedures 5.5.3 Experimental Results and Discussions 5.5.4 Determination of Shear Stress–Strain Curve References Problems

209 209 216 219 225 231 234 237 237 241 246 256 260 263

The Flow Theory of Plasticity 6.1 Introduction 6.2 The Concept of Yield Criterion 6.2.1 Mathematical Expressions of Yield Surface 6.2.2 Geometrical Representation of Yield Surface in the Principal Stress Space 6.3 The Flow Rule 6.4 The Elastic-Perfectly Plastic Material 6.5 Strain-Hardening 6.5.1 Drucker’s Postulate 6.5.2 The Isotropic-Hardening Rule 6.5.3 The Kinematic-Hardening Rule 6.5.4 General Form of Subsequent Yield Function and Its Flow Rule 6.6 The Return-Mapping Algorithm 6.7 Combined Axial–Torsion of Strain-Hardening Materials 6.8 Flow Theory in the Strain Space 6.9 Remarks References Problems

265 265 265 269

Advances in Plasticity 7.1 Introduction 7.2 Experimenal Determination of Yield Surfaces 7.2.1 Factors Affecting the Determination of Yield Surface 7.2.2 A Summary of Experiments Related to the Determination of Yield Surfaces 7.2.3 Yield Surface Versus Loading Surface 7.2.4 Yield Surface at Elevated Temperature 7.3 The Direction of the Plastic Strain Increment 7.4 Multisurface Models of Flow Plasticity

323 323 324

© 2005 by Chapman & Hall/CRC Press

271 274 276 286 287 290 296 301 306 308 314 316 317 318

325 328 333 335 336 340

Contents 7.4.1 The Mroz Kinematic-Hardening Model 7.4.2 The Two-Surface Model of Dafalias and Popov 7.5 The Plastic Strain Trajectory Approach 7.5.1 The Theory of Ilyushin 7.5.2 The Endochronic Theory of Plasticity 7.6 Finite Plastic Deformation 7.6.1 The Stress and Strain Measures 7.6.2 The Decomposition of Strain and Strain Rate 7.6.3 The Objective Rates 7.6.4 A Theory of Finite Elastic–Plastic Deformation 7.6.5 A Study of Simple Shear Using Rigid-Plastic Equations with Linear Kinematic Hardening 7.6.6 The Yield Criterion for Finite Plasticity References Problems 8

9

Internal Variable Theory of Thermo-Mechanical Behaviors and Endochronic Theory of Plasticity 8.1 Introduction 8.2 Concepts and Terminologies of Thermodynamics 8.2.1 The First Law of Thermodynamics 8.2.2 State Variables, State Functions, and the Second Law of Thermodynamics 8.3 Thermodynamics of Internal State Variables 8.3.1 Irreversible Systems 8.3.2 The Clausius–Duhem Inequality 8.3.3 The Helmholtz Formulation of Thermo-Mechanical Behavior 8.3.4 The Gibbs Formulation of Thermo-Mechanical Behavior 8.4 The Endochronic Theory of Plasticity 8.4.1 The Concepts of the Endochronic Theory 8.4.2 The Simple Endochronic Theory of Plasticity 8.4.3 The Improved Endochronic Theory of Plasticity 8.4.4 Derivation of the Flow Theory of Plasticity from Endochronic Theory 8.4.5 Applications of the Endochronic Theory to Metals 8.4.6 The Endochronic Theory of Viscoplasticity References Problems Topics in Endochronic Plasticity 9.1 Introduction 9.2 An Endochronic Theory of Anisotropic Plasticity 9.2.1 An Endochronic Theory Accounting for Deformation Induced Anisotropy 9.2.2 An Endochronic Theory for Anisotropic Sheet Metals

© 2005 by Chapman & Hall/CRC Press

ix 340 344 351 351 356 357 358 358 364 368 374 384 393 397 399 399 399 399 400 403 403 405 406 408 410 410 412 421 425 427 441 450 452 455 455 455 455 461

x

Contents 9.3

10

Endochronic Plasticity in the Finite Strain Range 9.3.1 Corotational Integrals 9.3.2 Endochronic Equations for Finite Plastic Deformation 9.3.3 Application to a Rigid-Plastic Thin-Walled Tube Under Torsion 9.4 An Endochronic Theory for Porous and Granular Materials 9.4.1 The Endochronic Equations 9.4.2 Application to Concrete 9.4.3 Application to Sand 9.4.4 Application to Porous Aluminum 9.5 An Endochronic Formulation of a Plastically Deformed Damaged Continuum 9.5.1 Introduction 9.5.2 The Anisotropic Damage Tensor 9.5.3 Gross Stress, Net Stress, and Effective Stress 9.5.4 An Internal State Variables Theory 9.5.5 Plasticity and Damage 9.5.6 The Constitutive Equations and Constraints 9.5.7 A Brief Summary of Wu and Nanakorn’s Endochronic CDM 9.5.8 Application 9.5.9 Concluding Remarks References Problems

468 469

Anisotropic Plasticity for Sheet Metals 10.1 Introduction 10.2 Standard Tests for Sheet Metal 10.2.1 The Uniaxial Tension Test 10.2.2 Equibiaxial Tension Test 10.2.3 Hydraulic Bulge Test 10.2.4 Through-Thickness Compression Test 10.2.5 Plane-Strain Compression Test 10.2.6 Simple Shear Test 10.3 Experimental Yield Surface for Sheet Metal 10.4 Hill’s Anisotropic Theory of Plasticity 10.4.1 The Quadratic Yield Criterion 10.4.2 The Flow Rule and the R-Ratio 10.4.3 The Equivalent Stress and Equivalent Strain 10.4.4 The Anomalous Behavior 10.5 Nonquadratic Yield Functions 10.6 Anisotropic Plasticity Using Combined Isotropic–Kinematic Hardening 10.6.1 Introduction

543 543 545 545 545 545 545 546 546 546 548 548 550

© 2005 by Chapman & Hall/CRC Press

474 476 487 490 500 502 503 506 506 507 512 516 521 523 526 530 535 537 541

552 553 555 558 558

Contents 10.6.2 The Anisotropic Theory Using Combined Isotropic–Kinematic Hardening 10.6.3 Results and Discussion 10.6.4 Summary and Conclusion References Problems 11

12

Description of Anisotropic Material Behavior Using Curvilinear Coordinates 11.1 Convected Coordinate System and Convected Material Element 11.2 Curvilinear Coordinates and Base Vectors 11.3 Tensors and Special Tensors 11.4 Multiplication of Vectors 11.5 Physical Components of a Vector 11.6 Differentiation of a Tensor with Respect to the Space Coordinates 11.6.1 Derivative of a Scalar 11.6.2 Derivatives of a Vector 11.6.3 Derivatives of a Tensor 11.7 Strain Tensor 11.8 Strain–Displacement Relations 11.9 Stress Vector and Stress Tensor 11.10 Physical Components of the Stress Tensor 11.11 Other Stress Tensors and the Cartesian Stress Components 11.12 Stress Rate and Strain Rate 11.13 Further Discussion of Stress Rate 11.14 A Theory of Plasticity for Anisotropic Metals 11.14.1 The Yield Function 11.14.2 The Flow Rule 11.14.3 The Strain Hardening 11.14.4 Elastic Constitutive Equations References Problems Combined Axial–Torsion of Thin-Walled Tubes 12.1 Introduction 12.2 Convected Coordinates in the Combined Axial–Torsion of a Thin-Walled Tube 12.3 The Yield Function 12.3.1 The Mises Yield Criterion 12.3.2 A Yield Criterion Proposed by Wu 12.4 Flow Rule and Strain Hardening 12.5 Elastic Constitutive Equations 12.6 Algorithm for Computation 12.7 Nonlinear Kinematic Hardening

© 2005 by Chapman & Hall/CRC Press

xi

560 566 572 575 577 579 579 580 584 590 591 592 593 593 594 599 603 606 609 610 612 617 619 621 628 628 629 630 631 633 633 634 637 637 638 642 646 647 649

xii

Contents 12.8 Description of Yield Surface with Various Preloading Paths 12.8.1 Path (1) — Axial Tension 12.8.2 Path (2) — Torsion 12.8.3 Path (3) — Proportional Loading 12.8.4 Tor–Ten Path (4) 12.8.5 Tor–Ten Path (5) 12.8.6 Tor–Ten Path with Constant Shear Strain 12.9 A Stress Path of Tension-Unloading Followed by Torsion 12.10 Summary and Discussion References Problems

Answers and Hints to Selected Problems

© 2005 by Chapman & Hall/CRC Press

649 652 656 660 660 662 664 665 668 669 670 671

Preface One of the aims of this book is to bring the subjects of continuum mechanics and plasticity together so that students will learn about the principles of continuum mechanics and how they are applied to the formulation of plasticity theory. Continuum Mechanics and Plasticity were traditionally two separate courses, and students had to make extra efforts to relate the two subjects in order to read the modern literature on plasticity. Another aim of this book is to include sufﬁcient background material about the experimental aspect of plasticity. Experiments are presented and discussed with reference to the veriﬁcation of theories. With knowledge of the experiments, the reader can make better judgments when realistic constitutive equations of plasticity are used. A third aim is to include anisotropic plasticity in this book. This important topic has not been fully discussed in most plasticity books on engineering mechanics. The ﬁnal aim of the book is to incorporate research results obtained by me and my coworkers related to the endochronic theory of plasticity, so that these results can be systematically presented and better understood by readers. Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (continuum) approach is still the practical approach for use in the simulation of engineering problems. Most current computations use a theory of plasticity for isotropic material and work with the Cauchy stress. However, material anisotropy has long existed in real structural components and machine parts. Its effect has mostly been neglected for the sake of computational simplicity, but material anisotropy does play a signiﬁcant role in the manufacturing process. A realistic description of material anisotropy may help reduce scraps in the manufacturing processes and reduce the amount of energy wasted. Also, components may be designed to possess certain predesigned anisotropy to enhance their performance. This book addresses the issue of material anisotropy by using the contravariant true stress that is deﬁned based on convected coordinates. A material element should be followed during anisotropic plastic deformation, where a square material element will no longer be square, and convected (curvilinear) coordinates should be used together with general tensors. The popular Cauchy stress is not useful in deﬁning the yield criterion, because it is deﬁned with respect to a rectangular Cartesian element. Even though recent works in computational mechanics have mostly been based on the Cartesian coordinate system, an understanding of the curvilinear coordinate system by computational mechanists and engineers will help develop computational algorithms suitable to addressing the issue of material anisotropy. Most books xiii

© 2005 by Chapman & Hall/CRC Press

xiv

Preface

that cover general tensors in curvilinear coordinates were published in the early 1960s and treat mainly elastic deformations. In this book, I devote a signiﬁcant number of pages to discussing a modern theory of plasticity using curvilinear coordinates. Recently published books address mainly computational methods and algorithms, neglecting the signiﬁcance of experimental study and material anisotropy. Their purpose is to discuss efﬁcient and stable methods and algorithms for analysis and design. In doing so, simple constitutive models are used for computational simplicity. Sometimes, unrealistic conditions, such as a nonsmooth yield function, have been discussed at length. A nonsmooth yield function has never been experimentally observed. Owing to tremendous advances in computer technologies and methods, computational power doubles and redoubles in a short time. Consequently, there will shortly be a demand for reﬁnements of constitutive models of plasticity. What is acceptable today will no longer be acceptable in the near future. At that time, an acceptable model will, among other things, be able to account for material anisotropy and produce results that compare well with experimental data. This book will help readers in meeting this challenge. I taught the subjects of continuum mechanics, elasticity, and plasticity in four separate semester-long courses at the University of Iowa from 1970 to 1986. During this period, the contents of these courses were constantly updated. Since 1987, I have been teaching a two-course series to replace these four courses. This new series essentially narrows down the coverage of continuum mechanics to solids (in the sense that no special treatment of ﬂuids and gases is included). However, it provides a more systematic and comprehensive coverage of the subject of the mechanics of solids. This book grew out of my lecture notes for the two-course series. There were three reasons for this change at the time, and these are still valid today. (1) A modern trend: Owing to recent advances in plasticity, the methods of continuum mechanics have been used to develop new theories of plasticity or to reformulate the existing theories. Therefore, in modern literature, continuum mechanics is essential to the understanding of plasticity. (2) Reduction of the number of courses offered: The original four courses have been reduced to two. Owing to budget constraints, it has been necessary for many engineering colleges, including the College of Engineering at the University of Iowa, to reduce the number of courses offered to students. (3) Suitability for students of computational solid mechanics: Owing to advances in computing technologies and methods, students of computational solid mechanics must use modern continuum mechanics and plasticity to obtain realistic numerical solutions to their engineering problems. These students need not only courses in continuum mechanics and plasticity but also courses that are oriented toward computation and data handling. The students are limited in terms of the number of courses that they can take but still need to learn the subjects well. The two-course series based on this book ﬁts the needs of this student group to integrate subject matter by the most efﬁcient means possible.

© 2005 by Chapman & Hall/CRC Press

Preface

xv

The book is divided into two parts: Part I — Fundamentals of Continuum Mechanics and Part II — Continuum Theory of Plasticity. Part I (Chapters 1 to 4) is suitable for use as a textbook at the ﬁrst-year graduate level for aerospace engineering, civil engineering, engineering mechanics, materials engineering, and mechanical engineering students. It is also suitable for use by advanced undergraduate students of applied mathematics. A second course may be taught to advanced graduate students from selected topics from Part II (Chapters 5 to 12). Since the book contains up-to-date materials, it may also be used by researchers and engineers as a reference book. The chapters are divided into sections and subsections. Technical terms are written in italic font when they ﬁrst appear. Examples are given within the text when further clariﬁcation is called for, and exercise problems are given at the end of each chapter. Mathematical fundamentals and Cartesian tensors are covered in Chapter 1; the concepts of the stress vector, the stress tensor, and stress invariants are discussed in Chapter 2; Chapter 3 discusses the kinematics of deformation; and Chapter 4 discusses the conservation laws, the constitutive equations, and elasticity. In this chapter, examples related to different stress measures are given. I have written Chapter 5 — Fundamentals of Continuum Plasticity from the viewpoint of an experimentalist with constitutive modeling in mind. The reader will acquire a general knowledge about different types of mechanical tests and the resulting material behavior in the small and large strain ranges. Potential sources of data uncertainty have been pointed out and discussed. In particular, I have discussed the hydrostatic pressure effect of yield stress and the assumption of plastic incompressibility. The reader will learn the classical ﬂow theory of plasticity in Chapter 6. I discuss recent advances in plasticity in Chapter 7, both experimentally and theoretically. In particular, I include ﬁnite plastic deformations with various objective rates and a discussion of yield surfaces determined using different stress measures. The fundamentals of endochronic theory are given in Chapter 8 and, in Chapter 9, I present topics of endochronic theory, which include anisotropic plasticity, ﬁnite strain, porous and granular materials, and a plastically deformed damaged continuum. Anisotropic plasticity is discussed further in Chapters 10 to 12. In Chapter 10, the discussion is of sheet metals. In Chapter 11, ﬁrst the fundamentals of the curvilinear coordinate system and general tensors and then the stress and strain with reference to the convected material element are discussed. Next different stress tensors and the stress rates are discussed. At the end of the chapter, a general theory of anisotropic plasticity is presented. Finally, in Chapter 12, the theory of Chapter 11 is applied to investigate the path-dependent evolution of the yield surface in the case of the combined axial-torsion of thin-walled tubes. I learned plasticity from the late Professor Aris Phillips of Yale University, who is well known for his life-time effort to determine yield surfaces. I then had the honor and privilege of working with Professor Kirk C. Valanis, who was a senior professor and departmental chair at Iowa during the 1970s. Professor Valanis is well known for his endochronic theory of plasticity, which

© 2005 by Chapman & Hall/CRC Press

xvi

Preface

at the time advocated a theory of plasticity without a yield surface. The years of working and having discussions with Kirk were most stimulating and inspiring, and he turned me into a disciple of his theory. As a result, I have spent most of my academic life in experimentally verifying and further developing the endochronic theory. During the same time, I have continued Professor Phillips’s efforts in the experimental determination of yield surface, and extended them into the large strain range. There is no doubt that yield surfaces can be experimentally determined, with some data scatter. It may be more appropriate to talk about a yield band with certain amounts of uncertainty than of a yield locus. The direction of plastic strain increment is, therefore, also associated with certain amounts of uncertainty. Kirk has since shown that yield surface can be derived from the endochronic theory in a limit case. I now view yield surface as a means of getting to an approximate solution of the problem at hand. Indeed, in many cases, a theory without a yield surface can have advantages in computation since all equations are continuous. I am indebted to the late Dr. Owen Richmond and to Dr. Paul T. Wang of Alcoa Laboratories for their continuing support of my research. The research support from the NSF, NASA, and the U.S. Army is also appreciated. I wish to express my sincere gratitude to the University of Iowa for the Career Development Award for the fall semester of the academic year 2001–2002. The award enabled me to plan for the book and start the initial part of my writing. My appreciation also extends to Professor David Y. Gao for his invitation to write this book and to Mr. Robert B. Stern, acquisitions editor and executive editor of CRC Press, for his assistance in publishing this book. Finally, I am thankful to my wife Yumi, whose love, encouragement, and patience enabled me to complete the writing of this book. Han-Chin Wu Iowa City, April 2004

© 2005 by Chapman & Hall/CRC Press

Author Professor Han-Chin Wu received his B.S. degree in civil engineering from National Taiwan University, his M.S. degree in structural engineering from the University of Rhode Island, and his M.S. and Ph.D. degrees in the mechanics of solids from Yale University. He has been teaching at the University of Iowa since 1970 and has supervised 19 Ph.D. students to completion. Dr. Wu is a professor in the Department of Civil and Environmental Engineering. He is also a professor of Mechanical Engineering and a fellow of American Society of Mechanical Engineers. His research interest is in the mechanical behavior (plastic ﬂow, damage, creep, fracture, and fatigue) of metals and porous and granular materials such as porous aluminum, concretes, ice, and soils. His methods are both experimental and theoretical in an effort at constitutive modeling. He is the author of 70 journal publications and more than 100 conference papers and research reports, and he has a patent on an axial– torsional extensometer for large strain testing.

xvii

© 2005 by Chapman & Hall/CRC Press

Part I

Fundamentals of Continuum Mechanics Continuum mechanics is a branch of mechanics concerned with stresses in solids, ﬂuids, and gas and the deformation or motion of these materials. A major assumption is that mass is continuous in a continuous medium and that the density can be deﬁned.

© 2005 by Chapman & Hall/CRC Press

1 Cartesian Tensors

1.1

Introduction

In this chapter, we discuss the basics of Cartesian tensors with the purpose of preparing the reader for subsequent chapters on continuum mechanics and plasticity. Curvilinear coordinates and general tensors as well as more advanced topics are discussed in Chapters 11 and 12. First, we discuss the notations in detail: both symbolic and index notations are used in this book. The symbolic notations simplify the equations and will help the reader in understanding the structure of the equations as the subscripts may be confusing. However, when a set of coordinate systems has been assigned, we utilize the index notation. We first discuss the tensor algebra, and then the differentiation and integration of tensors, which are standard materials. Some references [1–5] are given at the end of the chapter for additional reading.

1.1.1

Notations

In the symbolic notation, a vector is expressed by a bold-faced lowercase letter, say a, or by notations such as a, a, a, etc.; a tensor is expressed by a bold-faced ˜ such as A, A, A , etc. In the index notation, capital letter, say A, or by notations ˜ the components of a vector (the meaning of components will be discussed in Section 1.2.1) are denoted by ai , and the components of a second-rank tensor (discussed in Section 1.3.1) are denoted by Aij , or Tijk for a third-rank tensor. We note that a second-rank tensor has two subscripts, a third-rank tensor has three subscripts, and an nth-rank tensor has n subscripts. Summation and range conventions are used in the index notation. In the summation convention, a repeated index means summation of the term over the range of the index. For example, Akk = A11 + A22 + A33 , if the range of the index is from 1 to 3. On the other hand, if the range of the index is from 1 to n, then Akk = A11 + A22 + · · · + Ann , a sum of n terms. We note that the underscored n does not imply summation, and the index should not repeat more than once. The notation Akkk , for instance, is not deﬁned. The repeated index 3

© 2005 by Chapman & Hall/CRC Press

4

Continuum Mechanics and Plasticity

k is called a dummy index because it can be replaced by another index with no difference in its outcome. For example, Akk = Aii = Ajj = A11 + A22 + A33 . The range convention applies when there is a free (not repeated) index in a term. The free index takes a value of 1, 2, or 3 for a three-dimensional space. Equation yi = Cij xj is actually a set of three equations, and i is the free index. You may apply the range convention as follows: For i = 1,

y1 = C1j xj = C11 x1 + C12 x2 + C13 x3

For i = 2,

y2 = C2j xj = C21 x1 + C22 x2 + C23 x3

For i = 3,

y3 = C3j xj = C31 x1 + C32 x2 + C33 x3

(1.1)

Note that the summation convention has been applied in the last equality of each of the above equations.

1.1.2

Cartesian Coordinate System

We use (x1 , x2 , x3 ) instead of (x, y, z) to denote the axes of the Cartesian coordinate system. Sometimes, the coordinate axes may simply be denoted by 1, 2, and 3 in a ﬁgure. Using the index notation, the axes are xi . Throughout this book, the right-handed coordinate system will be used.

1.1.3

Special Tensors

There are two special tensors, δij and eijk , which are often used to simplify mathematical expressions. Kronecker’s delta δij is deﬁned as δij = 1

when i = j

=0

when i = j

(1.2)

Examples are δ11 = δ22 = δ33 = 1 and δ12 = δ21 = δ13 = δ23 = 0, etc. Using the summation convention, we ﬁnd δii = δ11 + δ22 + δ33 = 3. In the symbolic notation, Kronecker’s delta is a unit tensor 1, or it may be written as δ. A useful feature of Kronecker’s delta is its substitution property. We can then write δij aikp = ajkp , replacing i by j in the expression aikp . The permutation symbol eijk is also known as the alternating tensor, and it is deﬁned by

eijk

+1 = 0 −1

even permutation of 1, 2, 3 two or more subscripts are the same odd permutation of 1, 2, 3

(1.3)

Examples are e123 = e231 = e312 = 1, e321 = e132 = e213 = −1, and e112 = e133 = e111 = 0, etc.

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

1.2 1.2.1

5

Vectors Base Vectors and Components

In three-dimensional Euclidean space, the base vectors are e1 , e2 , and e3 . The base vectors are unit vectors in the Cartesian coordinate system and are not necessarily unit vectors in the curvilinear coordinate system (curvilinear coordinates are discussed in Chapter 11). In the Cartesian system, the base vectors are mutually perpendicular to each other. A vector a may be expressed as a = ap ep = a1 e1 + a2 e2 + a3 e3

(1.4)

where ap are the components of a relative to the basis ep . 1.2.2

Vector Addition and Multiplication

Vectors a and b may be added as follows: a + b = ap ep + bp ep = (ap + bp )ep

(1.5)

There are two kinds of multiplication, the scalar product and the vector product. The scalar product, also known as the dot product, of two base vectors ei and ej is ei · ej = δij

(1.6)

Examples are, when i = 1 and j = 2, e1 · e2 = 0, that is, e1 is perpendicular to e2 ; when i = 1 and j = 3, e1 · e3 = 0, which means that e1 is perpendicular to e3 . Generally, ei is perpendicular to ej for any permutation of i and j. The scalar product of vectors a and b is expressed by a · b = (ap ep ) · (bq eq ) = ap bq ep · eq = ap bq δpq = ap bp

(1.7)

The outcome of the scalar multiplication is also a scalar. Using this expression, the norm or the magnitude of vector a is given by |a| = [a · a]1/2 = [ap ap ]1/2

(1.8)

Thus, by use of (1.8), the norm of ei is one. The vector product is also known as the cross product. The outcome of a cross product is a vector. The cross products between Cartesian base vectors are e2 × e3 = e1 , e3 × e1 = e2 , e1 × e2 = e3 , which may be summarized by the following expression: ei × ej = ±eijp ep

© 2005 by Chapman & Hall/CRC Press

(1.9)

6

Continuum Mechanics and Plasticity

where the “+” sign applies for the right-handed coordinate system and the “−” sign applies for the left-handed coordinate system. Since the righthanded coordinate system will be used throughout this book, we will disregard the “−” sign from now on. By use of this notation, the cross product between vectors a and b becomes a × b = (ap ep ) × (bq eq ) = ap bq ep × eq = epqr ap bq er

(1.10)

Using the dot product, the components of a vector may be found as a · ei = ap ep · ei = ap δpi = ai

(1.11)

Therefore, vector a may be expressed as a = (a · ep )ep

(1.12)

The scalar triple product of vectors a, b, and c is a · (b × c) = ai ei · epqr bp cq er = epqr ai bp cq δir = epqr ar bp cq = epqr ap bq cr

(1.13)

The last expression of (1.13) was obtained by permutation of indices. The scalar triple product represents the volume of an element formed by vectors a, b, and c as its sides.

1.2.3

The e–δ Identity

The following identity is known as the e–δ identity. This identity has been frequently applied to provide simpliﬁed expressions in vector calculus. The identity is eijk eiqr = δjq δkr − δjr δkq

δ = jq δkq

δjr δkr

(1.14)

Note that i is summed. EXAMPLE 1.1

Prove the e–δ identity.

Proof We ﬁrst establish the identity

epqs emnr

© 2005 by Chapman & Hall/CRC Press

δmp = δnp δrp

δmq δnq δrq

δms δns δrs

(a)

Cartesian Tensors

7

To this end, we let T11 det T = T21 T31

T13 T23 T33

T12 T22 T32

(b)

Since an interchange of two rows in the determinant causes a sign change, we have Tm1 emnr det T = Tn1 Tr1

Tm3 Tn3 Tr3

Tm2 Tn2 Tr2

(c)

An interchange of columns causes a sign change too, and we also write T1p epqs det T = T2p T3p

T1s T2s T3s

T1q T2q T3q

(d)

For an arbitrary row and column interchange sequence, we can, therefore, write

emnr epqs

Tmp det T = Tnp Trp

Tmq Tnq Trq

Tms Tns Trs

(e)

When Tij = δij and det T = 1, the above equation is reduced to

emnr epqs

δmp = δnp δrp

δmq δnq δrq

δms δns δrs

(f)

which is the same as (a). The e–δ identity may then be obtained by setting m = p in (f). Expanding the resulting determinant on the right-hand side of the equation, this leads to emnr emqs = δmm (δnq δrs − δrq δns )− δmq (δnm δrs − δrm δns )+ δms (δnm δrq − δrm δnq ) = δmm (δnq δrs − δrq δns ) − 2(δnq δrs − δrq δns ) δ δ = δnq δrs − δrq δns = nq ns δrq δrs which is the e–δ identity given by (1.14).

© 2005 by Chapman & Hall/CRC Press

(g)

8

Continuum Mechanics and Plasticity

EXAMPLE 1.2 The e–δ identity may be applied to prove other identities. An example is to prove the following identity:

a × (b × c) = b(a · c) − c(a · b)

Proof LHS = ai ei × (bj ej × ck ek ) = ai ei × (erjk bj ck er ) = erjk ai bj ck (ei × er ) = erjk esir ai bj ck es = erjk ersi ai bj ck es = (δjs δki − δji δks )ai bj ck es = δjs δki ai bj ck es − δji δks ai bj ck es = ai bj ci ej − ai bi ck ek = (ai ci )bj ej − ck ek (ai bi ) = RHS Similarly, the following identities may be proven: a · (b × c) = (a × b) · c (a × b) · (c × d) = (a · c)(b · d) − (a · d)(b · c) (a × b) × (c × d) = b[a · (c × d)] − a[b · (c × d)]

1.3

The Transformation of Axes

Consider the rectangular Cartesian coordinate system x1 , x2 , and x3 shown in Figure 1.1. If we rotate the coordinate system through some angle about its origin O, the new coordinate axes become x1 , x2 , and x3 . The direction cosines between xi and xj are Qij = cos(xi , xj )

(1.15)

where the ﬁrst subscript denotes the unprimed axes and the second subscript the primed axes. In general, Qij = Qji , e.g., Q23 = Q32 ,

or

cos(x2 , x3 ) = cos(x3 , x2 ).

In the matrix form, we write Qij as

Q11 [Q] = Q21 Q31

© 2005 by Chapman & Hall/CRC Press

Q12 Q22 Q32

Q13 Q23 Q33

(1.16)

Cartesian Tensors

9 x3

x′3 x′2 A

e3 e′3

e′2 x2

e2

O

e⬘1 e1 x′1 x1 FIGURE 1.1 Transformation of coordinate systems.

We now discuss the properties of the transformation matrix [Q]. From vector −→ analysis and referring to Figure 1.1, the unit vector OA is expressed as −→ −→ −→ −→ OA = cos(x1 , OA)e1 + cos(x2 , OA)e2 + cos(x3 , OA)e3

(1.17)

−→ If we take OA along the x1 direction, and denote the vector by e 1 , then (1.17) becomes e 1 = cos(x1 , x1 )e1 + cos(x2 , x1 )e2 + cos(x3 , x1 )e3 = Q11 e1 + Q21 e2 + Q31 e3 = Qj1 ej

(1.18)

Equation (1.18) shows that Qj1 are direction cosines for the unit vector e 1 . −→ Since the magnitude of OA is one, we write 2 2 2 Q11 + Q21 + Q31 =1

or

Qi1 Qi1 = 1

(1.19)

−→ Similarly, if we take OA along the x2 direction and denote the vector by e 2 , we obtain 2 2 2 Q12 + Q22 + Q32 =1

© 2005 by Chapman & Hall/CRC Press

or

Qi2 Qi2 = 1

(1.20)

10

Continuum Mechanics and Plasticity

−→ Again, if we take OA along the x3 direction and denote the vector by e 3 , we get 2 2 2 + Q23 + Q33 =1 Q13

or

Qi3 Qi3 = 1

(1.21)

A general form of equation (1.18) is e i = Qji ej

(1.22)

Since e i and e j (i = j) are perpendicular to each other, their dot products are zero. Therefore, from (1.22), e i · e j = (Q1i e1 + Q2i e2 + Q3i e3 ) · (Q1j e1 + Q2j e2 + Q3j e3 ) = Q1i Q1j + Q2i Q2j + Q3i Q3j = 0

(1.23)

and we obtain Qki Qkj = 0

i = j

for

(1.24)

Summarizing (1.19)–(1.21) and (1.24), we write Qki Qkj = δij

(1.25)

When i = j, (1.25) reduces to (1.19)–(1.21); and when i = j, (1.25) reduces to (1.24). In the matrix notation, we then have [Qik ]T [Qkj ] = [δij ]

or simply

[Q]T [Q] = [1]

(1.26)

Note that [Qik ]T = [Qki ] is the transpose of matrix [Qik ]. When performing matrix multiplication, the summation convention is used adjacently, that is, a dummy index is used for two adjacent subscripts in matrix multiplication. Equation (1.26) is an important relationship. The matrix [Q] is orthogonal, which will be discussed further in Section 1.6.1. In a similar manner, we can show that Qik Qjk = δij

or

[Q][Q]T = [1]

(1.27)

−→ This is accomplished by taking unit vector OA along x1 , x2 , and x3 , respectively, and ﬁnding projections of ei on the xi axes. Thus, ei = Qi1 e 1 + Qi2 e 2 + Qi3 e 3 = Qij e j

(1.28)

and the magnitude of the vector is Qik Qik = 1

© 2005 by Chapman & Hall/CRC Press

for

i = 1, 2, 3

(1.29)

Cartesian Tensors

11

If we consider the dot products between ei and ej , we obtain Qik Qjk = 0

i = j

for

(1.30)

The above two equations lead to (1.27). We rewrite (1.22) and (1.28) here to emphasize their importance in the transformation of axes: e i = Qji ej

(1.22)

ei = Qij e j

(1.28)

and

These are equations relating the base vectors of the primed and unprimed coordinate systems. In (1.22), QijT transforms a unit vector ei into the unit vector e i and, in (1.28), Qij transforms the unit vector e i back into ei . The direction cosines Qki may also be obtained from ek · e i = ek · Qji ej = δkj Qji = Qki

(1.29)

The transformation formula for vector a is a = a i e i = aj ej = aj Qji e i

or

a i = Qji aj

(1.30)

or, in the matrix form, [a ] = [Q]T [a]

(1.31)

The inverse relation of (1.31) is obtained by writing a = aj ej = a i e i = a i Qji ej

or

ai = Qij a j

(1.32)

or, in the matrix form, [a] = [Q][a ]

(1.33)

Note that the same Qij is used in both relations (1.31) and (1.33). Finally, we note that the scalar product of vectors a and b is a · b = a i b i = Qji aj Qki bk = δjk aj bk = aj bj = ai bi

(1.34)

We see from (1.34) that the value of a · b is independent of the coordinate system to which the components are referred. A quantity with such a property is called an invariant.

© 2005 by Chapman & Hall/CRC Press

12

1.4

Continuum Mechanics and Plasticity

The Dyadic Product (The Tensor Product)

Some physical quantities require the speciﬁcation of two vectors for their description. Quantities of this kind can be described by a dyadic product. The dyadic product of two vectors u and v is written as u ⊗ v. It has the associative and distributive properties given by (αu) ⊗ v = u ⊗ (αv) = α(u ⊗ v) u ⊗ (v + w) = u ⊗ v + u ⊗ w,

(v + w) ⊗ u = v ⊗ u + w ⊗ u

(1.35)

where α is a scalar. In terms of the components of u and v, u ⊗ v may be written as u ⊗ v = (ui ei ) ⊗ (vj ej ) = ui vj ei ⊗ ej = u1 v1 e1 ⊗ e1 + u1 v2 e1 ⊗ e2 + u1 v3 e1 ⊗ e3 + u 2 v1 e2 ⊗ e 1 + u 2 v2 e2 ⊗ e 2 + u 2 v3 e2 ⊗ e 3 + u 3 v1 e3 ⊗ e 1 + u 3 v2 e3 ⊗ e 2 + u 3 v3 e3 ⊗ e 3

(1.36)

The components of u ⊗ v are ui vj , which can be displayed in a matrix:

u 1 v1 [u ⊗ v] = u2 v1 u3 v1

u1 v2 u2 v2 u3 v2

u1 v3 u2 v3 u3 v3

(1.37)

The dyadic products ei ⊗ ej of the base vectors ei are called unit dyads. Thus, the dyadic product u ⊗ v is expressed in (1.36) in terms of its components ui vj and its bases ei ⊗ ej . The form of (1.36) is independent of the choice of the coordinate system. Using (1.22, 1.27, 1.30), we obtain u i vj e i ⊗ e j = Qpi up Qqj vq Qri er ⊗ (Qsj es ) = Qpi Qri Qqj Qsj up vq er ⊗ es = δpr δqs up vq er ⊗ es = ur vs er ⊗ es = ui vj ei ⊗ ej

(1.38)

In general, the commutative law is not valid, that is, u ⊗ v = v ⊗ u. An additional property of a dyadic product is that it forms an inner product with a vector. We may take the following relations as deﬁnitions: (u ⊗ v) · w = u(v · w),

u · (v ⊗ w) = (u · v)w

(1.39)

u · v ⊗ w = (u · v)w

(1.40)

These relations may also be written as u ⊗ v · w = u(v · w),

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

13

since there is no possibility of ambiguity. We see in (1.39) and (1.40) that an inner product of a dyadic product with a vector yields another vector. The concept of a dyadic product can be extended to products of three or more vectors. Thus, the product of three vectors u, v, and w is a triad and is written u ⊗ v ⊗ w. Similarly, we can deﬁne tetrads or higher-order polyads. The triad u ⊗ v ⊗ w in its component form is written as ui vj wk ei ⊗ ej ⊗ ek .

1.5 1.5.1

Cartesian Tensors General Properties

We deﬁne a second-rank (order) Cartesian tensor as a linear combination of dyadic products. Since, from (1.36), a dyadic product is itself a linear combination of unit dyads, a second-rank Cartesian tensor T can be expressed as a linear combination of unit dyads. This deﬁnition of a Cartesian tensor is equivalent to deﬁning the tensor as a linear transformation that transforms a vector into another vector. We see from (1.39) that u ⊗ v transforms a vector into another vector and, from (1.35), that it obeys the associative and distributive properties of a linear transformation. Therefore, u ⊗ v is a tensor. In the component form, tensor T is written as T = Tij ei ⊗ ej = T11 e1 ⊗ e2 + T12 e1 ⊗ e2 + T13 e1 ⊗ e3 + T21 e2 ⊗ e1 + · · · (1.41) The coefﬁcients Tij are called the components of T. We will denote tensor components by the same letter that we use to denote the tensor itself and remark that a tensor exists independently of any coordinate system. Its components can only be speciﬁed after a coordinate system has been chosen, and the values of the components depend on the choice of the coordinate system. If, in a new coordinate system with base vectors e i , tensor T has components Tij , then from (1.41)

T = Tij ei ⊗ ej = Tpq ep ⊗ e q

(1.42)

Tij ei ⊗ ej = Tij Qip Qjq e p ⊗ e q

(1.43)

But, by use of (1.28),

Therefore, by equating the above two equations, their coefﬁcients are related by

Tpq = Qip Qjq Tij

© 2005 by Chapman & Hall/CRC Press

or

T Tpq = Qpi Tij Qjq

(1.44)

14

Continuum Mechanics and Plasticity

This is the transformation formula for components of second-rank tensors. Equation (1.44) may also be considered as an alternative deﬁnition of a secondrank tensor. In order to identify a second-rank tensor as such, we may show that its components transform according to (1.44) from one coordinate system, xi , to another, xi . The nine components of Tij may be displayed in a 3×3 square matrix [T], so that the above equation may be written in a matrix equation as [T ] = [Q]T [T][Q].

(1.45)

The matrix form is often convenient for algebraic manipulation. We now extend the relation (1.41) to express a Cartesian tensor of rank (order) n in terms of components as T = Tij···m ei ⊗ ej ⊗ · · · ⊗ em

(1.46)

Note that the components Tij...m have n indices and the tensor product has n factors. The components of this nth-rank tensor transform according to the rule

Tpq...t = Qip Qjq · · · Qmt Tij...m

(1.47)

From this more general viewpoint, a scalar can be interpreted as a tensor of rank zero, since it has a single component which is unchanged in a coordinate transformation; a vector is considered as a tensor of rank one. Most of the tensors we encounter in this book will be of rank zero (scalars), one (vectors), or two. We will also discuss some fourth-rank tensors due to their importance in continuum mechanics. The inverse relation to (1.44) is

Tij = Qip Qjq Tpq

or

T Tij = Qip Tpq Qqj

(1.48)

Or, in the matrix form, it is written as [T] = [Q][T ][Q]T

(1.49)

We also note that the inverse of (1.47) is

Tij...m = Qip Qjq · · · Qmt Tpq...t

(1.50)

For a second-rank tensor T, the transpose of T is deﬁned as TT = Tij ej ⊗ ei = Tji ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

(1.51)

Cartesian Tensors

15

Tensor T is symmetric if T = TT . Thus, from (1.41) and (1.51), we ﬁnd Tij = Tji for a symmetric T. With reference to the xi system, we have, from (1.44),

= Qiq Qjp Tij = Qjp Qiq Tji = Tpq Tqp

(1.52)

which proves the symmetry with respect to the primed coordinate system. We may conclude that if a tensor is symmetric with reference to one Cartesian system, then it has symmetric components with reference to all Cartesian coordinate systems. Similarly, if T = −TT , then Tij = −Tji , and T is an antisymmetric second-rank tensor. An antisymmetric tensor has components

0 −T12 −T13

T12 0 −T23

T13 T23 0

(1.53)

Finally, we remark that any second-rank tensor can be decomposed into the sum of a symmetric and an antisymmetric tensor, and that this decomposition is unique. We write T = 21 (T + TT ) + 21 (T − TT )

(1.54)

The tensor (T + TT ) is symmetric and the tensor (T − TT ) is antisymmetric. We also mention that an identity tensor I is a special case, where Tij = δij . Thus, the identity tensor is written as I = e1 ⊗ e1 + e2 ⊗ e2 + e3 ⊗ e3

(1.55)

T·I=T

(1.56)

with

EXAMPLE 1.3 Show that an arbitrary tensor A can be expressed as the sum of a spherical tensor (i.e., a scalar times the identity tensor) and a tensor with zero trace (trace A = Aii ). Prove that this decomposition is unique, and that A , the traceless part of A, is given by A = A − 13 (tr A)I, where A is the deviator of A.

Solution Deﬁne B = A − 13 (tr A)I

and

C = 13 (tr A)I

(a)

then A=B+C

© 2005 by Chapman & Hall/CRC Press

(b)

16

Continuum Mechanics and Plasticity

and C is a spherical tensor. We now take the trace of the ﬁrst equation of (a) and get tr B = tr{A − 13 (tr A)I} = tr A − tr 13 (tr A)I = tr A − 13 (tr A)(3) = 0

(c)

Therefore, B is traceless, and from (b) A is the sum of a spherical tensor and a traceless tensor. To prove the uniqueness, we ﬁrst assume that this decomposition is not unique. Then, there exists a spherical tensor D and a traceless tensor E such that A=D+E

(d)

We take the trace of (d) and (b) to ﬁnd tr A = tr D + tr E = tr D = tr C

(e)

because E and B are traceless. Since both D and C are spherical tensors, we write D = DI

and

C = CI

(f)

where both D and C are scalars. Using (e) and taking the trace of (f), we ﬁnd D = C, that is, D = C. This leads to E = B, which proves that the decomposition is unique.

1.5.2

Multiplication of Tensors

Consider a vector s = si ei and a second-rank tensor T = Tij ei ⊗ ej in a coordinate system with base vectors ei . In a new system with base vectors e i = Qji ej , vector s and tensor T have components s i and Tij , respectively, so that s i = Qmi sm ,

Tij = Qri Qsj Trs

(1.57)

The outer product of the vector s and the tensor T is deﬁned by W = s ⊗ T = si ei ⊗ Tjk ej ⊗ ek = si Tjk ei ⊗ ej ⊗ ek = Wijk ei ⊗ ej ⊗ ek

(1.58)

Therefore, the outer product is a third-rank tensor with components given by Wijk = si Tjk . Referring to the new coordinate system, we write

W = s ⊗ T = s i Tjk e i ⊗ e j ⊗ e k = Wijk ei ⊗ e j ⊗ e k

© 2005 by Chapman & Hall/CRC Press

(1.59)

Cartesian Tensors

17

= s T . If we substitute e = Q e into the above equation, we Hence, Wijk ji j i jk i can establish the following transformation formula for the components Wijk :

Wijk = Qpi Qrj Qsk Wprs

(1.60)

We note that the order of multiplication is important and that s ⊗ T = T ⊗ s. Similarly, the outer product of second-rank tensors P and S is R = P ⊗ S = Pij ei ⊗ ej ⊗ Skm ek ⊗ em = Pij Skm ei ⊗ ej ⊗ ek ⊗ em = Rijkm ei ⊗ ej ⊗ ek ⊗ em

(1.61)

and the components are Rijkm = Pij Skm . R is a fourth-rank tensor. In a similar manner, we may form the outer products of three or more tensors or vectors. The outer product of a tensor of rank p with a tensor of rank q is a tensor of rank p + q. We note that the dyadic product of two vectors is a special case, because vectors are tensors of rank one. If we equate the last two indices of third-rank tensor Wijk , we obtain

Wijj = Wi11 + Wi22 + Wi33

(1.62)

in which i is a free index and can take values of i = 1, 2, 3. Using the components transformation formula, we have

Wijj = Qpi Qrj Qsj Wprs = Qpi δrs Wprs = Qpi Wprr

(1.63)

Thus, the components Wprr transform as the components of a vector. This operation of reducing the rank of tensor by two by summing on two indices is called contraction of the tensor. In (1.63), a third-rank tensor is reduced to a vector by contraction. In the case of a tensor of rank n with components Wijkm...rs , if we sum on any pair of its indices such as k = r, then the resulting quantities Wijrm...rs , are the components of a tensor of rank n − 2. In particular, contraction of a second-rank tensor Tij leads to Tii , a scalar. The outer product followed by a contraction leads to an inner product. The inner product of vector s and tensor T is s · T = si Tik em ⊗ em ⊗ ek = si Tik ek

(1.64)

where the relation em ⊗ em = I is applied, in which I is the identity tensor. The inner product formed by a different order is T · s = Tij sj ei ⊗ em ⊗ em = Tij sj ei = si Tki ek

(1.65)

Comparing the two equations given above, we see that s · T = T · s only if T is a symmetric tensor. A similar procedure may be applied to form inner

© 2005 by Chapman & Hall/CRC Press

18

Continuum Mechanics and Plasticity

products of second- and higher-rank tensors. From second-rank tensors U and V, various inner products can be formed, such as U · V = Uij Vjk ei ⊗ ek ,

UT · V = Uji Vjk ei ⊗ ek

(1.66)

These inner products are second-rank tensors. A useful relation involving the inner product is (U · V)T = VT · UT

(1.67)

Using the concept of inner product, we may derive an expression for the components Tij of a second-rank tensor T. Based on (1.41), we may form the following inner product ei · T · ej = ei · Tpq ep ⊗ eq · ej = Tpq ei · ep ⊗ eq · ej = Tpq ei · ep (eq · ej ) = Tpq ei · ep δqj = Tpq δip δqj = Tij

(1.68)

Therefore, the component Tij of tensor T is given by Tij = ei · T · ej

(1.69)

It can be further shown that, from (1.69), we can obtain the following expression T · ej = Tpj ep

1.5.3

(1.70)

The Component Form and Matrices

Matrix operation can be conveniently used to perform transformation of tensor components from one coordinate system to another. For this purpose, we express a tensor equation in terms of a matrix equation in this section. Consider w =T·v

(1.71)

where T transforms vector v into vector w. This equation may be written as wi ei = T · vj ej = vj Tij ei

(1.72)

Thus, the components of (1.72) may be arranged in a matrix equation as [wi ] = [Tij ][vj ]

© 2005 by Chapman & Hall/CRC Press

(1.73)

Cartesian Tensors

19

where wi and vi may be arranged as the elements of two 3 × 1 column matrices [wi ] = [w1 , w2 , w3 ]T , [vi ] = [v1 , v2 , v3 ]T , whereas [Tij ] is a 3 × 3 square matrix. In the case of equation R =S·T

(1.74)

where R, S, and T are second-rank tensors, we write R · ei = S · T · ei

(1.75)

By use of (1.70), we have Rji ej = S · (Tji ej ) = Tji (S · ej ) = Tji Skj ek

or

Rki ek = Tji Skj ek

(1.76)

The component form is now Rki = Skj Tji

(1.77)

[Rik ] = [Sij ][Tjk ]

(1.78)

and the matrix form is

1.5.4

Quotient Law

The quotient law may be used to test whether the elements of a set of quantities A(i, j, k) are components of a tensor. If the inner product (summation over i) between A(i, j, k) and an arbitrary tensor, say bi , is known to yield a tensor Cjk , that is, A(i, j, k)bi = Cjk

(1.79)

then A(i, j, k) is a tensor of type Aijk . Referring to the xi coordinate system, the above equation is written as

A (i, j, k)b i = Cjk

(1.80)

are both tensors, they obey tensor transformation rules given Since b i and Cjk by (1.30) and (1.44), respectively. By substitution, we obtain

A (i, j, k)b i = Qpj Qqk Cpq = Qpj Qqk A(r, p, q)br = Qpj Qqk A(r, p, q)Qri b i

(1.81)

or [A (i, j, k) − Qri Qpj Qqk A(r, p, q)]b i = 0

© 2005 by Chapman & Hall/CRC Press

(1.82)

20

Continuum Mechanics and Plasticity

Since b i is an arbitrary tensor and is generally not zero, we conclude that the quantity within the brackets must vanish. Therefore, A (i, j, k) = Qri Qpj Qqk A(r, p, q)

(1.83)

which is the transformation rule for a tensor of type Aijk . This method may be used to test higher rank tensors.

1.6 1.6.1

Rotation of a Tensor Orthogonal Tensor

The inverse to tensor T is denoted by T−1 , so that T · T−1 = I

and

T−1 · T = I

(1.84)

In the case that the transpose of T is equal to the inverse of T, that is, TT = T−1

(1.85)

then T is said to be an orthogonal tensor. Therefore, for an orthogonal tensor, we have T · TT = I and

TT · T = I

with

det T = ±1

(1.86)

where the “+” sign denotes a proper orthogonal transformation (righthanded coordinate system) and the “−” sign denotes an improper orthogonal transformation (left-handed coordinate system). We now consider the transformation tensor Q discussed in Section 1.3. Since Q satisﬁes (1.86), it is an orthogonal tensor. For the purpose of investigating physical properties of Q, consider two vectors u and v transformed by Q: u¯ = Q · u,

v¯ = Q · v

(1.87)

The inner products Q · u and Q · v may be viewed as linear transformations of vectors u and v by tensor Q. The scalar product of u and v is u¯ · v¯ = (Q · u) · (Q · v) = v · QT · (Q · u) = u · v

(1.88)

which is unchanged under an orthogonal transformation Q. The second equality in (1.88) was a result obtained from the deﬁnition of the transpose of a tensor given by a · (AT · b) = b · (A · a).

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

21

A special case of the above discussion is u = v and u¯ = v. ¯ Here, (1.88) reduces to v¯ · v¯ = (Q · v) · (Q · v) = v · v

(1.89)

|v| ¯ = |v|

(1.90)

or

Therefore, the magnitude of a vector is unchanged by an orthogonal transformation. Furthermore, the angle φ between the two vectors is expressed by cos φ =

u·v u¯ · v¯ = |u||v| |u|| ¯ v| ¯

(1.91)

which means that the angle between the vectors is also unchanged. Thus, an orthogonal transformation rotates a vector and the components Qij are the direction cosines. EXAMPLE 1.4

Show that (Q · u) · (Q · v) = u · v.

LHS = (Qij ei ⊗ ej · uk ek ) · (Qmn em ⊗ en · vp ep ) = Qij Qmn uk vp ei δjk em δnp = Qij uj Qmn vn δim = Qij Qin uj vn = δjn uj vn = uj vj = u · v = RHS Deﬁne the transpose of tensor A by a · (AT · b) = b · (A · a) and shows that it leads to

EXAMPLE 1.5

(AT )T = A. By use of (1.65), we have LHS = a · (ATij bj ei ) = ak ek · ATij bj ei = ak ATij bj δki = ai ATij bj RHS = b · (Aij aj ei ) = bk ek · Aij aj ei = bk Aij aj δki = bi Aij aj = aj Aij bi = ai Aji bj Since the two sides are equal, we obtain ATij = Aji , that is, the transpose of a matrix is the same as the interchange of the two indices. We then have (ATij )T = Aij and we can write AT = ATij ei ⊗ ej = Aji ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

and

(AT )T = Aij ei ⊗ ej = A

22 1.6.2

Continuum Mechanics and Plasticity Component Form of Rotation of a Tensor

In this section, we derive the component form that describes the rotation of a tensor, and we point out that this transformation equation is different from the one which describes the change of bases. In the case of transformation of bases, it has been shown in Sections 1.2.3 and 1.2.5 that the components transform by [vi ] = [Qij ]T [vj ]

[vi ] = [Qij ][vj ]

and

(1.92)

for a vector vi , and by [Tij ] = [Qip ]T [Tpq ][Qqj ]

and

[Tij ] = [Qip ][Tpq ][Qqj ]T

(1.93)

for a tensor Tij . By applying rotation Q to vector v, we write v¯ = Q · v

(1.94)

Thus, vector v is rotated by Q into v. ¯ If the same Q has rotated the bases ei into e i , we can write v¯ = v¯ i e i = Q · v = Q · vi ei = vi (Q · ei ) = vi e i

(1.95)

v¯ i = vi

(1.96)

Therefore,

Equation (1.96) shows that the components of v¯ in e i are the same as those of v in ei . This result is obvious, because both the vector and the coordinate system have been rotated by the same amount and their relative positions remain the same. Consider next the components of v¯ in ei : v¯ = v¯ i ei = Q · v = Q · vi ei = vi Qji ej = vj Qij ei

(1.97)

[v¯ i ] = [Qij ][vj ]

(1.98)

Thus,

Note that this equation is different from (1.92). Equation (1.92) describes the components of v in the e i system, while (1.98) describes the components of the rotated vector v¯ in the ei system. The inverse relation of (1.98) is [vi ] = [Qij ]T [v¯ j ]

© 2005 by Chapman & Hall/CRC Press

(1.99)

Cartesian Tensors

23

We now apply Q to tensor T and write T¯ = Q · T · QT

(1.100)

that is, T¯ is the tensor after rotation. Then, T¯ · e i = T¯ ji e j = Q · T · QT · e i = Q · T · ei = Q · Tji ej = Tji e j

(1.101)

Thus, T¯ ji = Tji

(1.102)

that is, the components of T¯ in e i are the same as those of T in ei , when e i and ei are related by Q. To ﬁnd the component of T¯ with respect to ei , we write T¯ · e i = Q · T · QT · e i = Q · T · ei = Q · Tji ej = Tji Qkj ek

(1.103)

On the other hand, we have T¯ · e i T¯ · Q · ei = T¯ · Qji · ej = Qji T¯ · ej = Qji T¯ kj ek

(1.104)

Equating (1.103) to (1.104), we ﬁnd Qji T¯ kj = Tji Qkj

(1.105)

Multiplying both sides of the equation by Qmi , the resulting equation reduces to T¯ ij = Qim Qjn Tmn

(1.106)

which, in the matrix form, may be written as ¯ = [Q][T][Q]T [T]

(1.107)

Note that this equation (1.107) is different from (1.93) in that the latter describes the components of T in the e i system, while the former describes the components of the rotated tensor T¯ in the ei system.

1.6.3 1.6.3.1

Some Remarks Remark 1 — deﬁnition of Qij

In this book, we deﬁne the components of the transformation matrix by Qij = cos(xi , xj ), in which the ﬁrst subscript refers to the unprimed axis and

© 2005 by Chapman & Hall/CRC Press

24

Continuum Mechanics and Plasticity

the second subscript to the primed axis. The transformation rule for a second-rank tensor T is Tij = Qki Qmj Tkm

(1.108)

In some books, the following equations are used, Tij = Qik Qjm Tkm

(1.109)

where the transformation matrix is deﬁned by Qij = cos(xi , xj ). In this case, the ﬁrst subscript refers to the primed axis and the second subscript to the unprimed axis. Make a note of this difference. 1.6.3.2 Remark 2 — transformation of bases versus rotation of a tensor Note the difference in the transformation equations between a tensor T subjected to the transformation of bases and the tensor T itself undergoing rotation. In the transformation of bases Tij = Qki Qlj Tkl

or

[T ] = [Q]T [T][Q]

(1.110)

and in the rotation of a tensor ¯ = [Q][T][Q]T [T]

(1.111)

For rotation of tensor T in the reversed direction, we substitute [Q] by [Q]T ¯ = [Q]T [T][Q] which is the same as the result and (1.111) reduces to [T] obtained from the rotation of bases. Therefore, rotation of the tensor itself in the opposite direction has the same effect as the rotation of bases. This point is illustrated by Example 1.6. Consider the rotation of a vector v through an angle α into v. ¯ Observing that the magnitude of the vector remains the same in the rotation, that is, |v| ¯ = |v| and, from Figure 1.2, referring to ei , we can write

EXAMPLE 1.6

v¯ 1 = |v| cos(α + β) = |v|(cos α cos β − sin α sin β)

v1 v2 = |v| cos α − sin α = v1 cos α − v2 sin α |v| |v|

(a)

v¯ 2 = |v| sin(α + β) = |v|(sin α cos β + cos α sin β)

v1 v2 = |v| sin α + cos α = v1 sin α + v2 cos α |v| |v|

(b)

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

25 x2 _ v

_ v2 v2

v _ v1

O

v1

x1

FIGURE 1.2 Components of a vector.

We may then use equations (a) and (b) in a matrix equation as v¯ 1 cos α = sin α v¯ 2

− sin α cos α

v1 v2

(c)

The component form of this rotation is from (1.98) v¯ i = Qij vj

(1.98)

Comparing (c) and (1.98), we ﬁnd

cos α sin α

Qij =

− sin α cos α

(d)

However, a rotation of coordinate axes through an angle α in the opposite direction leads to

cos α sin α Qij∗ = (e) − sin α cos α Therefore, from equations (d) and (e), we obtain [Q∗ ]T = [Q]

(f)

The transformation formula in this case is, from (1.92), vi = Qji∗ vj = Qij∗T vj

(g)

Hence, v1 v2

© 2005 by Chapman & Hall/CRC Press

=

cos α sin α

− sin α cos α

v1 v2

(h)

26

Continuum Mechanics and Plasticity

Comparing (c) and (h), we conclude that rotation of a vector through an angle α has the same effect as rotation of axes through the same angle α in the opposite direction. Note that in using (1.98) to obtain v¯ i , the rotation matrix [Q] is obtained by rotating the coordinate axes through angle α in the same direction as the rotation of vector v.

1.6.3.3 Remark 3 — rotation of a vector about an arbitrary direction We now consider the rotation of a vector v about an arbitrary direction with unit vector n and denoted by OA (Figure 1.3(a)). The angle of rotation is α in the sense of the rotation of a right-handed screw advancing in the direction ¯ of n. In the rotation, vector v is rotated into v¯ and particle P is rotated into P. ¯ Hence, P and P lie in a plane normal to line OA, and the plane intersects OA at B. The vector of OB is bn and the length BP = BP = s. From the ﬁgure, we obtain b = n · v = n · v¯

(1.112)

We denote vectors BP and BP by s and s¯ , respectively. Thus, v = bn + s

and

v¯ = bn + s¯

(1.113)

¯ the unit vectors u = s/s and u¯ = s¯ /s are related by In the plane of BPP, u¯ = u cos α + n × u sin α

(1.114)

which can be easily justiﬁed from Figure 1.3(b). Equation (1.114), when multiplied by s, is s¯ = s cos α + n × s sin α (1.115) (a)

(b)

A x3 _ s

B

bn

_

O

_

cos u

P v

v

x2

x1

FIGURE 1.3 Rotation of (a) a vector about a direction; (b) a unit vector.

© 2005 by Chapman & Hall/CRC Press

u

sin

s

_ P

Cartesian Tensors

27

Substituting (1.115) into (1.113), we obtain v¯ = bn + s cos α + n × s sin α = bn + (v − bn) cos α + n × (v − bn) sin α = v cos α + n × v sin α + b(1 − cos α)n = v cos α + n × v sin α + (n · v)(1 − cos α)n

(1.116)

This equation may be written as follows in the component form: v¯ i = vi cos α + eikj nk vj sin α + (1 − cos α)vj nj ni

(1.117)

By comparing with (1.98), we ﬁnd that Qij = δij cos α + eikj nk sin α + (1 − cos α)ni nj

(1.118)

which is the rotation matrix describing the rotation of α about the line OA. In a special case, a rotation about the x3 -axis is obtained by setting n3 = 1 and n1 = n2 = 0 in (1.118) and we obtain

cos α Qij = sin α 0

− sin α cos α 0

0 0 1

(1.119)

A rotation in a reverse sense is denoted by a rotation of −α. In this case, (1.118) gives Qij∗ = δij cos(−α) + eikj nk sin(−α) + (1 − cos(−α))ni nj = δij cos α − eikj nk sin α + (1 − cos α)ni nj = Qji = QijT

(1.120)

Thus, we have shown that a rotation in the reverse sense (−α) can be represented by the transpose of the orthogonal tensor Q, which describes the original rotation (+α). Finally, we note that if the angle α is small, cos α ≈ 1 and sin α ≈ α. Then, equation (1.118) reduces to Qij = δij + αnk ekji

(1.121)

1.6.3.4 Remark 4 — symbolic versus component form Relations between tensor quantities may be expressed either in symbolic or in component form. The former are relations between scalars α, β, . . ., vectors u, v, . . ., and tensors R, S, . . ., and the latter are relations between scalars α, β, . . ., vector components ui , vi , . . ., and tensor components Rij , Sij , . . .. The symbolic notation has the advantage that it emphasizes that the relations are physical

© 2005 by Chapman & Hall/CRC Press

28

Continuum Mechanics and Plasticity

statements and that they are independent of the choice of the coordinate system. On the other hand, the component form is often convenient for carrying out algebraic manipulations. In solving problems, it is always necessary at some stage to introduce a coordinate system and components.

1.7

The Isotropic Tensors

A tensor is isotropic if it has the same components with respect to a Cartesian coordinate system of any orientation. Isotropic tensors of various ranks are given below: Scalar: Every scalar is an isotropic tensor, because the scalar does not have a direction. Vector: There is no nontrivial isotropic vector. Second-rank tensor: The general expression for an isotropic second-rank tensor is Tij = λδij

(1.122)

where λ is a constant. Third-rank tensor: The isotropic third-rank tensor is Tijk = λeijk

(1.123)

Fourth-rank tensor: The most general expression for an isotropic fourthrank tensor is Tijkm = αδij δkm + βδik δjm + γ δim δjk

(1.124)

where α, β, and γ are constants. If Tijkm has the symmetry properties that Tijkm = Tjikm and Tijkm = Tijmk , then from (1.124) Tijkm = Tjikm = αδij δkm + βδjk δim + γ δjm δik = αδij δkm + βδik δjm + γ δim δjk

(1.125)

By subtracting the two expressions in (1.125), and multiplying the resulting equation by δim δjk , we obtain δim δjk γ (δjm δik − δim δjk ) = β(δik δjm − δjk δim )δim δjk

© 2005 by Chapman & Hall/CRC Press

(1.126)

Cartesian Tensors

29

which may be further simpliﬁed to yield γ (δii − δii δjj ) = β(δii − δjj δii )

(1.127)

γ =β

(1.128)

or

Hence, (1.124) may be further reduced to Tijkm = αδij δkm + β(δik δjm + δim δjk )

(1.129)

and we see that the independent constants are now reduced to α and β. EXAMPLE 1.7

Show that there are no nontrivial isotropic vectors.

Proof Introduce a 180◦ rotation of the coordinate system about the x1 -axis as shown in Figure 1.4(a). The transformation matrix for this rotation of axes is

1 [Q] = 0 0

0 −1 0

0 0 −1

(a)

The transformation equation for a vector a is a i = Qji aj . By applying (a), this equation becomes a1 1 a 0 = 2

0 a3 x3

(a)

T 0 a1 a1 0 a2 = −a2 −1 a3 −a3

0 −1 0

x3

(b)

(b)

(c)

x3, x3⬘

x1⬘ x2⬘

O

x2

x1, x1⬘

O

x1 x3⬘

x2, x2⬘

x3⬘

O x1 d x1⬘

d x2

x⬘2

FIGURE 1.4 An 180◦ rotation of coordinate system about (a) the x1 -axis, (b) the x2 -axis, and (c) rotation of a small angle dθ about the x3 -axis.

© 2005 by Chapman & Hall/CRC Press

30

Continuum Mechanics and Plasticity

But, if a vector is isotropic, then a i = ai by deﬁnition. To satisfy this requirement and equation (b), we must have a2 = a3 = 0. However, coordinate axes may be labeled in an arbitrary order. Therefore, a1 = 0 as well. We conclude that there are no nontrivial isotropic vectors.

EXAMPLE 1.8

Tij = λδij .

Show that the isotropic second-rank tensor is given by

Proof Consider a 180◦ rotation of the coordinate system about the x1 -axis (see Figure 1.4(a)). The transformation equation for a second-rank tensor

= Q Q T . By applying (a) of Example 1.7, this equation becomes T is Tpq ip jq ij

T11 [T ] = −T21 −T31

−T12 T22 T32

−T13 T11 T23 = [T] = T21 T33 T31

T12 T22 T32

T13 T23 T33

(a)

The last equality of the above equation is written based on the deﬁnition of an isotropic tensor so that Tij = Tij . Therefore, we conclude that T12 = T21 = 0 and T13 = T31 = 0. We next introduce a 180◦ rotation of the coordinate system about the x2 -axis as shown in Figure 1.4(b). The transformation matrix is

−1 [Q] = 0 0

0 1 0

0 0 −1

(b)

Substituting (b) into the transformation equation for Tij and considering the deﬁnition of an isotropic tensor, we write

T11 [T ] = −T21 T31

−T12 T22 −T32

T13 −T23 T33

isotropic

≡

[T]

(c)

From (c), we conclude that T12 = T21 = 0 and T23 = T32 = 0. Thus, only T11 , T22 , T33 are nonzero. But, since coordinate axis may be labeled in any arbitrary order, we have T11 = T22 = T33 = λ. Therefore, the second-rank isotropic tensor is written as Tij = λδij

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors EXAMPLE 1.9

31

Show that the most general fourth-order isotropic tensor has

the form Tijkm = αδij δkm + βδik δjm + γ δim δjk where α, β, γ are constants. Proof A fourth-order tensor transforms as

Tijkm = Qri Qsj Qtk Qnm Trstn

(a)

There are 34 = 81 components altogether. First, consider any component which contains the index 1 only once. For the coordinate transformation associated with a 180◦ rotation about the x1 -axis and illustrated by Figure 1.4(a), the transformation matrix is given by (a) of Example 1.7. Let i = 1 and use the Qij of Figure 1.4(a), equation (a) becomes

= Qr1 Qsj Qtk Qnm Trstn = Q11 Qsj Qtk Qnm T1stn T1jkm

(b)

But j = 1, so the only nonzero terms of Qsj are Q22 = Q33 = −1, in which j = s; k = 1, so the only nonzero terms of Qtk are Q22 = Q33 = −1, in which k = t; and m = 1, so the only nonzero terms of Qnm are Q22 = Q33 = −1, in which m = n. Thus, (b) becomes

T1jkm = Q11 (−1)(−1)(−1)T1stn = −T1stn = −T1jkm

(c)

= T1jkm , which contradicts the expresIf the tensor is isotropic, then T1jkm sion in (c). Therefore, all the components which contain the index 1 only once are zero, in order to satisfy this requirement. Similarly, all the components that contain the index 2 only once are zero and all the components that contain the index 3 only once are zero. Thus, from the above special transformation, we see that the components of Tijkm are reduced to the following four groups: T1122 , T2211 , T1133 , . . . ; T1212 , T2323 , . . . ; T1221 , T2112 , T2332 , . . . ; and T1111 , T2222 , T3333 . Furthermore, we remark that the coordinate axes may be labeled in an arbitrary order. Thus, a permutation of the indices 1, 2, 3 cannot affect the values of the components of an isotropic tensor. Therefore,

T1122 = T2211 = T1133 = T3311 = T2233 = T3322 = α, say T1212 = T2121 = T1313 = T3131 = T2323 = T3232 = β, say T1221 = T2112 = T1331 = T3113 = T2332 = T3223 = γ , say T1111 = T2222 = T3333 = δ, say

© 2005 by Chapman & Hall/CRC Press

(d)

32

Continuum Mechanics and Plasticity

Consider now a rotation shown in Figure 1.4(c) about the x3 -axis with a very small angle of rotation dθ. The transformation matrix for this case is

cos dθ Qij = sin dθ 0

− sin dθ cos dθ 0

0 1 0 ≈ dθ 1 0

−dθ 1 0

0 0 1

(e)

Equation (e) can be rewritten as

1 Qij = 0 0

0 1 0

0 0 0 + dθ 1 0

−dθ 0 0

0 0 0

or Qij = δij + dθ e3ji

(f)

Only e321 and e312 are not zero in the expressions of e3ji . Note that (f) can also be obtained from (1.121) by letting ni = (0, 0, 1) and α = dθ . Substituting (f) into (a), we have

= (δri + dθ e3ir )(δsj + dθ e3js )(δtk + dθe3kt )(δnm + dθ e3mn )Trstn Tijkm

= (δri δsj + δri dθ e3js + dθ e3ir δsj )(δtk δnm + δtk dθ e3nm + dθ e3kt δnm )Trstn = (δri δsj δtk δnm + δri δsj δtk dθε3mn + δri δsj dθ e3kt δnm + δri dθ e3js δtk δnm + dθ e3ir δsj δtk δnm )Trstn = Tijkm + dθ e3mn Tijkn + dθ e3kt Tijtm + dθe3js Tiskm + dθ e3ir Trjkm = Tijkm + dθ {e3mn Tijkn + e3kt Tijtm + e3js Tiskm + e3ir Trjkm }

(g)

In the above derivation higher order terms in dθ have been neglected since

= Tijkm . Using this dθ is inﬁnitesimal. If the tensor Tijkm is isotropic, then Tijkm information in the last expression of (g), the quantity within the brackets has to be zero. Therefore, e3mn Tijkn + e3kt Tijtm + e3js Tiskm + e3ir Trjkm = 0

(h)

We now investigate the implication of (h). By choosing i = 1, j = k = m = 2, (h) becomes e321 T1221 + e321 T1212 + e321 T1122 + e312 T2222 = 0 or T2222 = T1221 + T1212 + T1122

© 2005 by Chapman & Hall/CRC Press

(i)

Cartesian Tensors

33

Substituting (d) into (i), we get δ =α+β +γ

(j)

Other choices of indices i, j, k, m in (h) gives either the same relation (j) or relations that are identically satisﬁed, if we use the isotropy conditions previously obtained. Thus, we have shown that there are only three distinct components of an isotropic fourth-rank tensor, namely α, β and γ ; and Tijkm can be written as Tijkm = αδij δkm + βδik δjm + γ δim δjk

(k)

All components of isotropic Tijkm can be found from (k). Examples are T1122 = αδ11 δ22 + βδ12 δ12 + γ δ12 δ12 = α T2233 = αδ22 δ33 + βδ23 δ23 + γ δ23 δ23 = α T1221 = αδ12 δ21 + βδ12 δ21 + γ δ11 δ22 = γ and so on. EXAMPLE 1.10 Using the expression of an isotropic fourth-rank tensor, reduce the generalized Hooke’s law to an isotropic relation. Linearly elastic materials are governed by the generalized Hooke’s law as

σij = Cijkm εkm

(a)

where σij and εij are second-rank tensors and Cijkm is a fourth-rank tensor. Due to the symmetric property of σij and εij , we ﬁnd Cijkm = Cjikm and Cijkm = Cijmk . If the material is isotropic, tensor Cijkm should be an isotropic tensor. Thus, from (1.130), Cijkm = λδij δkm + µ(δik δjm + δim δjk )

(b)

Substituting (b) into (a), we obtain σij = λδij δkm εkm + µδik δjm εkm + µδim δjk εkm = λεkk δij + µεij + µεji = λδij εkk + 2µεij

(c)

In the derivation, the symmetric property of εij = εji was used. λ and µ are known as Lamé constants.

© 2005 by Chapman & Hall/CRC Press

34

1.8 1.8.1

Continuum Mechanics and Plasticity

Vector and Tensor Calculus Tensor Field

If to every point xi of region R there corresponds a scalar φ, then we have a scalar ﬁeld φ(xi ) deﬁned over R. An example of the scalar ﬁeld is the temperature ﬁeld, where the temperature in the region R of a continuum is known and may vary from point to point. Similarly, we can deﬁne a vector ﬁeld. If to every point xi of region R corresponds a vector vi , then we have a vector ﬁeld vi (xj ) deﬁned over R. Force ﬁeld, displacement ﬁeld, and velocity ﬁeld are examples of vector ﬁeld. A tensor ﬁeld can be similarly deﬁned. Stress ﬁeld and strain ﬁeld are tensor ﬁelds of rank two.

1.8.2

Gradient, Divergence, Curl

We consider differentiation and integration in the study of vector calculus. Differentiation is discussed in this section and integration in a later section. There are three kinds of differentiation: the gradient, the divergence, and the curl. The gradient of a scalar ﬁeld φ, denoted by Grad φ, is a vector whose components are Grad φ =

∂φ ∂φ ∂φ , , ∂x1 ∂x2 ∂x3

T

= a vector

(1.130)

In other notations, Grad φ may be denoted by −−−−→ ∂φ Grad φ = ek = φ,i ek = ∇φ ∂xk

(1.131)

“del” is used in the last expression of (1.131). In our The differential operator ∇ notation ∇ is = ek ∂ ∇ ∂xk

(1.132)

is not commutative with respect to the quantity which it The operator ∇ operated in the sense that = φ ∇ ∇φ

(1.133)

1.8.2.1 Geometric signiﬁcance of the gradient The value of the scalar ﬁeld φ(xk ) deﬁned over the region R varies in general with xi . The expression, φ(xk ) = constant, deﬁnes a set of surfaces on which φ

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

35

P(xi ) ∆xi

x3

Surface S on which is Constant

x2

O

P⬘(xi + ∆xi)

x1 FIGURE 1.5 A constant φ surface.

is constant. Consider a point P(xi ) and a neighboring point P (xi + xi ) on the surface S, and denote the vector from P to P by xi as shown in Figure 1.5. Since both points are on the same surface, φ evaluated at the two points are the same, and we write φ(P ) − φ(P) = 0

or φ(xi + xi ) − φ(xi ) = 0

(1.134)

Expanding the function φ(xi + xi ) in Taylor’s series, we have φ(xi + xi ) = φ(xi ) + φ,i xi + 0(xi )2

(1.135)

But, xi has a small value and we may take it as small as possible in the sense of calculus. In this way, we may neglect the higher order terms in xi and keep only the ﬁrst-order term in (1.135). Therefore, (1.134) becomes φ(P ) − φ(P) = φ,i xi = 0

(1.136)

and this is true for any vector xi through P lying on the surface S. Hence, the gradient φ,i is normal to the surface S. 1.8.2.2 Differential operators on vectors There are two differential operators on vector vi which are well known. They are the divergence and the curl. The divergence of vector v is written as Div v ≡ vi,i =

∂vi = ∂xi

∂v1 ∂v2 ∂v3 + + ∂x1 ∂x2 ∂x3

(1.137)

the divergence is In terms of ∇, · v = ek Div v = ∇

© 2005 by Chapman & Hall/CRC Press

∂ ∂vm · (vm em ) = ek · em = δkm vm,k = vk,k ∂xk ∂xk

(1.138)

36

Continuum Mechanics and Plasticity

The curl of vector v, denoted by vector w, is × v = ek ∂ × (vm em ) = ek × ej vj,k = ekjm em vj,k w = Curl v = ∇ ∂xk

(1.139)

and its components are Wm = (Curl v)m = ekjm vj,k = emkj vj,k

(1.140)

in which vj,k is the velocity gradient if vi is the velocity. The velocity gradient is an important kinematic quantity and is discussed in Chapter 3. From (1.140), we have w1 = v3,2 − v2,3 . Vector wm is the dual vector of tensor vj,k except for a constant multiple factor. Dual vectors are discussed in Chapter 3. are given below: Some operations using the operator ∇ (a) (b)

∂ · (∇φ) ∇ = ej · (ek φ,k ) = ej · ek φ,kj = δjk φ,kj = φ,kk = ∇ 2 φ ∂xj × (∇φ) = Curl Grad φ = ej ∂ × (ek φ,k ) = ej × ek φ,kj ∇ ∂xj

(1.141)

= ejkm em φ,kj = ejk1 e1 φ,kj + ejk2 e2 φ,kj + ejk3 e3 φ,kj = e231 e1 φ,32 + e321 e1 φ,23 + · · · = 0

(1.142)

We note that ejk1 is antisymmetric and φ,kj is symmetric such that their inner product is zero. For the same reason the other two terms involving m = 2 and m = 3 are also zero. The above result can also be seen easily by expanding out each term as in the last equality. Since e231 = 1 and e321 = −1, the terms of the last equality cancel out in pairs. (c)

∂ ∂ ∇ · (∇ × v) = ej · ek × (er vr ) ∂xj ∂xk = ej

∂ ∂ · [ek × er vr,k ] = ej · [ekrs vr,k es ] ∂xj ∂xj

= ej · ekrs es vr,kj = δjs ekrs vr,kj = ekrj vr,kj = 0

(1.143)

The last equality is again obtained by observing that the inner product of an antisymmetric tensor with a symmetric tensor is zero. (d)

× (∇ × v) = es ∂ × [ekjm vm,j ek ] = es × ek ekjm vm,js ∇ ∂xs = −eksr er ekjm vm,js = −{δsj δrm − δsm δrj }vm,js er = −vm,ss em + vs,js ej = −vm,ss em + (vs,s ),j ej ∇ · v) = −∇ 2 v + ∇(

© 2005 by Chapman & Hall/CRC Press

(1.144)

Cartesian Tensors

37

Note that ∇ 2 v is written as:

2 · ∇)v = ei ∂ · ej ∂ (vk ek ) = ∂ vk (ei · ej )ek (∇ ∂xi ∂xj ∂xi ∂xj =

∂ 2 vk ek = vk,jj ek ∂xj ∂xj

(1.145)

By use of (1.39), we have · ∇)v = v⊗∇ ·∇ (∇

(1.146)

Therefore, ∇ 2 v can be written in either of the following two forms ·∇ = (∇ · ∇)v ∇ 2v = v ⊗ ∇

(1.147)

(e) There are two forms of the divergence of tensor T. They are: ∂Tpq ∂Tpq · T = ∂ ek ·(Tpq ep ⊗ eq ) = ∇ (ek · ep )eq = eq ∂xk ∂xk ∂xp = T·∇

∂Tqp eq ∂xp

(1.148)

(1.149)

The two divergences are in general different, but they are the same if the =∇ ·T, and this relationship tensor T is symmetric. We can further write TT · ∇ is similar to that of the inner product between a vector and a second-rank tensor presented in (1.64) and (1.65).

1.8.3

The Theorem of Gauss

In continuum mechanics, an important application of the theorem of Gauss is to change an area integral into a volume integral and vice versa. Consider a body of surface S and volume V, with surface element dS and volume element dV shown in Figure 1.6, the Gauss theorem is written as S

φni dS =

S

φ,i dV

for scalar φ

(1.150)

vj ni dS =

S

V

V

vj,i dV

ai1 i2 ...iN nj dS =

© 2005 by Chapman & Hall/CRC Press

for vector vj

(1.151)

V

ai1 i2

... iN ,j

dV

for tensor ai1 ...iN

(1.152)

38

Continuum Mechanics and Plasticity

dV nAi

ni

A

dS P ui

P⬘ B

x3

nBi x2

O x1

FIGURE 1.6 Surface and volume elements in a deformable body.

Proof We prove (1.150) here. The proofs of (1.151) and (1.152) can be similarly obtained. Ascalar ﬁeld φ is deﬁned in V and we divide the body into an inﬁnite number of parallel inﬁnitesimal cylinders. A generic inﬁnitesimal cylinder is shown in the Figure 1.6 with ends Aand B. Ends Aand B are parts of the surface B area S of the body and has unit outward normal nA i or ni , respectively. We

now consider two neighboring points P(xi ) and P (xi +dxi ) in the inﬁnitesimal cylinder. The unit vector along the generator of the cylinder is denoted by ui as shown in the Figure 1.6 and is a constant. The differential dφ is given by

dφ =

∂φ ∂φ ∂φ dx1 + dx2 + dx3 = φ,i dxi = ui φ,i ds ∂x1 ∂x2 ∂x3

(1.153)

where ds is the length of dxi . If this expression is integrated over the inﬁnitesimal cylinder, we ﬁnd φB − φA = ui

B A

φ,i ds

(1.154)

The cross-section of the cylinder is dT = (−ni ui dS)A = (ni ui dS)B

© 2005 by Chapman & Hall/CRC Press

(1.155)

Cartesian Tensors

39

Note that ni ui is negative at A and positive at B. Multiplying both sides of (1.154) by (1.155), we obtain φB (ni ui dS)B − φA (−ni ui dS)A = ui

B

φ,i ds dT

(1.156)

φ,i dV

(1.157)

A

which may be rewritten as (φni ui dS)B + (φni ui dS)A = ui

B A

or ui

dSA +dSB

φni dS = ui

Vcylinder

φ,i dV

(1.158)

In deriving (1.158), we observe that because dSA and dSB are small surface areas, we assume that φ and ni are constants in dS, then ui

dSA +dSB

φni dS = ui

dSA

φni dS + ui

∼ = ui (φni )A

dSA

dSB

φni dS

dS + ui (φni )B

dS dSB

= (φni ui dS)A + (φni ui dS)B = LHS of (1.157)

(1.159)

Equation (1.158) is valid for the inﬁnitesimal cylinder considered. For the whole body, we sum over all inﬁnitesimal cylinders and obtain

Sall

φni dS =

Vall

φ,i dV

(1.160)

which proves equation (1.150). We remark that the theorem of Gauss is still valid for multiply connected region. In that case, we have to make branch cuts to prove the theorem. Some special cases of the theorem are listed below: 1. Expressions in 3-D: V

Div v dV =

© 2005 by Chapman & Hall/CRC Press

S

n · v dS

(divergence theorem)

(1.161)

40

Continuum Mechanics and Plasticity S

n

L FIGURE 1.7 Contour and surface.

This equation can be obtained by putting i = j in (1.151).

V

Curl v dV =

S

n × v dS

(1.162)

This equation can be obtained by multiplying both sides of (1.152) by ekij . 2. Expressions in 2-D: S

Div v dS =

L

n · v dL

Curl v dS = n × v dL S L v · dL = n · Curl v dS (Stoke’s theorem) L

(1.163) (1.164) (1.165)

S

In the two-dimensional case, the theorem changes the surface integral into the line integral and vice versa. Figure 1.7 shows the contour L and the surface S. In (1.165), the left integral is the circulation of v along the contour L and n is the unit outward normal on the surface S.

References 1. Malvern, L.E., Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Englewood Cliffs, NJ, 1969. 2. Spencer, A.J.M., Continuum Mechanics, Longman, London and New York, 1980. 3. Lai, W.M., Rubin, D., and Krempl, E., Introduction to Continuum Mechanics, Pergamon Press, New York, 1974. 4. Fung, Y.C., First Course in Continuum Mechanics, Prentice-Hall, Englewood Cliffs, NJ, 1994. 5. Chadwick, P., Continuum Mechanics, George Allen & Unwin, London, 1976.

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

41

Problems (1) The equations of motion are ∂Tsr + ρbr = ρar ∂xs Write out the equations in conventional notations, that is, use x = x1 , y = x2 and z = x3 . (2) Prove that δij δij = 3 eijk Aj Ak = 0 δij eijk = 0 (3) If Tij is symmetric, evaluate the expressions (a) eijk Tjk and (b) eijk eist Tkt . (4) Given that

1 [Sij ] = −1 2

0 3 −1

0 2 1

evaluate (a) Sii , (b) Sjj , (c) Sij Sij , (d) Sjk Skj , (e) Smn Snm (5) Using the e–δ identity, show that eikm ejkm = 2δij

and

eijk eijk = 6

(6) Given vectors u = ui ei and v = vi e, show that the components of w = u×v are w1 = u2 v3 − u3 v2 ,

w2 = u3 v1 − u1 v3 ,

w3 = u1 v2 − u2 v1

(7) If ui = eijk vj wk and vi = eijk sj tk , show that ui = sk wk ti − tk wk si . (8) Find the transformation matrix [Q] if the coordinate system is rotated through a positive 90◦ about the positive x3 -axis. (9) Can the matrices

1 0 0

0 2 0

0 0 3

and

be matrices of the same tensor? Why?

© 2005 by Chapman & Hall/CRC Press

1 0 0

0 1 0

0 0 3

42

Continuum Mechanics and Plasticity

(10) The components of a second-rank tensor with respect to the xi coordinate system are

4 [A] = 3 0

3 −1 0

0 0 1

Find the components of the same tensor with respect to the xi , coordinate system, if x3 = x3 and x1 is making a 30◦ counterclockwise angle with the x1 -axis. (11) Prove that the decomposition of a tensor into a symmetric and an antisymmetric part is unique. (12) Show that the value of Aij xi xj is unchanged if Aij is replaced by its symmetric part. (13) If Aij is a tensor and Bij is a symmetric tensor, show that the product Aij Bij is independent of antisymmetric part of Aij . (14) In the coordinate transformation from xi to xi , the transformation rule for the

= Q Q T , where Q is the transcomponents of a second-rank tensor is Tpq ip jq ij ij formation matrix. Derive the reversed expression of this equation, that is, express Tij in terms of Tij and Qij . (15) Investigate the inﬂuence of the coordinate transformation x1 = −x1 , x2 = x2 , x3 = x3 on the components of a tensor T. (16) Prove that ei ⊗ ei = I where I is the identity tensor. (17) Show that det(ei ⊗ ei ) = 1 and det(e1 ⊗ e1 ) = 0. (18) Show that (a ⊗ b) · (c ⊗ d) = (b · c)(a ⊗ d). (19) Show that if the components of tensor T are Tij = δij in the xi coordinate system, then the components are Tij = δij in the xi coordinate system. (20) A rigid body is rotated through positive 90◦ about x2 -axis by the right-handed screw rule. Find a matrix representing this rotation. (21) Suppose that the body of the previous problem is subsequently given a 90◦ rotation about the x1 -axis by the right-hand screw rule, ﬁnd the matrix representation of the resultant rotation. If the position of a particle P on the rigid body was (0, 1, 1), what is its position after two rotations? (22) Reverse the order of above two rotations and ﬁnd the ﬁnal position of P. (23) A rigid body undergoes two rotations. The ﬁrst is a rotation through a positive 30◦ angle about a direction speciﬁed by the unit vector n = 0.286e1 +0.857e2 + 0.429e3 with respect to a ﬁxed Cartesian coordinate system with origin at O. This rotation is followed by a second rotation which rotates a positive 90◦ angle about a direction speciﬁed by the unit vector m = −0.667e1 −0.667e2 +0.333e3 . Both axes of rotation pass through the origin O. If the position of a point P on the rigid body is (1, 1, 0), what is its position after the two rotations?

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

43

(24) The velocity ﬁeld vi (x) of a rigid body can be written as vi = bi + eijk cj xk , where the vectors bi and cj do not depend on the position of the considered particle. Show that the curl of this velocity ﬁeld is 2ci while the divergence of the velocity ﬁeld vanishes. (25) In the vector ﬁeld v(x), let there exist a surface on which v = 0. Show that, at an arbitrary point of this surface, Curl v is tangential to the surface or vanishes, while Div v is given by the rate of change of the normal component of v in the direction of the normal of the surface. (26) A tensor M transforms every vector into its mirror image with respect to the plane whose normal is √ 2 n= (e + e2 ) 2 1

(a) Find the matrix of M. (b) Use this linear transformation to ﬁnd the mirror image of a vector a = e1 + 2e2 . (Note that this is not a case of rotation. This case is known as reﬂection.) (27) Let φ(x, y, z) and ψ(x, y, z) be scalar functions of positions, and let v(x, y, z) and w(x, y, z) be vector functions of position. By writing in the component form, verify the following identities: + ψ) = ∇φ + ∇ψ (a) ∇(φ (b) Div(v + w) = Div v + Div w · v + φ(Div v) (c) Div(φw) = (∇φ) (28) Consider the integral L e3ij ni vj dL, where L is the closed boundary of a plane surface S with normal (0, 0, 1); vi is a vector; ni is the outward normal of the contour L. Show that this integral is the circulation of vector vi along L denoted by L v · dL.

© 2005 by Chapman & Hall/CRC Press

2 Stress

2.1

Introduction

When forces are applied to a body, they cause the body to deform. In this chapter, we study about the forces and the intensity of forces, and in the next chapter, we study the deformation of the body. The intensity of forces is known as stress, and it is the stress, not the force, that plays an important role in the quantiﬁcation of effect due to forces. A force may be applied to a small area, and a distributed load of the same resulting magnitude may be applied to a larger area. The effects of the two cases are different locally because the stresses are not the same. The concept of stress needs to be deﬁned, and it can be represented by a second-rank tensor. We investigate the properties of stress in this chapter and we also list some references [1–6] for additional reading.

2.2

Forces

Consider a body of volume V and surface S as shown in Figure 2.1. A generic material element of the body has a volume dV, and a generic surface element has area dS and an outward normal n. There are four types of “forces” that act on a body. The “forces” include, in a broad sense, the forces and moments. The four types of “forces” are: 1. Body forces: These are forces whose magnitudes are proportional to the mass contained in the material element of the body. The body forces may either be deﬁned per unit mass or per unit volume. An important example of body force is the gravity force, which is expressed as ρg dV, where ρ is the density; and g is the gravitational acceleration. 2. Surface forces: These forces act on the surface element dS of the body. Externally applied loads, contact forces between bodies, and reactions are examples of surface forces, out of which surface tractions or stress vectors may be deﬁned. The stress vector is the stress force per unit area. 45

© 2005 by Chapman & Hall/CRC Press

46

Continuum Mechanics and Plasticity

dV

t(n)

b dS

r

n

x3

x2

O x1 FIGURE 2.1 Body force and surface traction.

3. Body moments: These are moments applied to the volumetric element dV. It is usually expressed in terms of moment per unit volume, or moment per unit mass. 4. Couple stress: The couple stress is the moment per unit area applied on a surface. In this chapter, we consider only the ﬁrst two types of forces — body and surface forces. These are the most common forces that appear in the study of thermo-mechanical behavior of engineering materials. The remaining two types of “forces” are not important in the case of mechanical behavior of materials, but they play an important role in the case of a polarized dielectric solid under the action of an electric ﬁeld. They also could be signiﬁcant in the study of bones or materials with microstructures, and/or from the action of an external magnetic ﬁeld. Even without external couples, couple stress can arise from interactions between adjacent parts of the material other than central-force interaction. In this chapter, we study the basic principles and methods of continuum mechanics.

2.3

Stress Vector

The stress vector is also known as the surface traction. Consider the surface element dS shown in Figure 2.1, where the surface force applied to the element is p. We write p = t(n) dS

© 2005 by Chapman & Hall/CRC Press

(2.1)

Stress

47

where p dS→0 dS

t(n) (xk ) = lim

(2.2)

where t(n) is the stress vector, which is the intensity of surface force and has a unit of force per unit area. The stress vector is a function of position, a function of xi , and in general it is different from one point on the surface of the body to another point. The outward normal of dS is denoted by n, and t(n) and n are not in the same direction.

2.4

The Stress Tensor

We now consider the stress inside the body, let us cut out a tetrahedron of inﬁnitesimal size from a body, as shown in Figure 2.2. The triangular surface dS(n) , with outward normal n, is inclined to the coordinate axes. The remaining three sides of the tetrahedron, dS1 , dS2 , and dS3 , lie on the coordinate surfaces, and their outward normals are −e1 , −e2 , and −e3 , respectively. The stress vectors acting on these surfaces are −t1 , −t2 , and −t3 , respectively. The negative sign indicates that these forces act on the surfaces with negative normals. Let us now consider the force equilibrium of the tetrahedron. For this we need to sum the surface forces acting on all faces of the tetrahedron and the body force ρb dV acting on the mass of the tetrahedron and then set the result to zero. We obtain −t1 dS1 − t2 dS2 − t3 dS3 + ρb dV + dS(n) t(n) = 0 x3 –t1

t(n)

∆S1 O –t2

n

∆S2

x2 ∆S

3

∆S (n)

∆V b –t3 x1 FIGURE 2.2 Stress vectors.

© 2005 by Chapman & Hall/CRC Press

(2.3)

48

Continuum Mechanics and Plasticity

On applying a limiting process, the volume dV tends to zero, but successive smaller elements retain their surfaces parallel. Since the volume and the area are of the third order and the second order of smallness in length, respectively, in the limit, the term ρb dV becomes a higher order of smallness relative to the other terms and can be ignored. Thus, (2.3) becomes t1 dS1 + t2 dS2 + t3 dS3 = dS(n) t(n)

(2.4)

Since dSi are projections of the inclined surface dS(n) onto the coordinate surfaces, we have dSi = ni = cos(xi , n) dS(n)

(2.5)

By use of (2.5), (2.4) reduces to t(n) = ti ni

(2.6)

Referring to (2.6), we emphasize that t(n) is a vector acting on the inclined surface dS(n) , and ti are vectors acting on the surfaces dSi . Each of these vectors can be expressed by its components referred to the coordinate axes xi . To do this, we write (n)

t(n) = tk ek

and

ti = σik ek

(2.7)

(n)

where tk are the components of t(n) ; and σik are the components of ti in the coordinate directions. Substituting (2.7) in (2.6), we obtain (n)

tk ek = σik ek ni

or

(n)

tk = σik ni

(2.8)

which, in the matrix form, is written as [t(n) ] = [σ ]T [n]

(2.9)

The quantities σik are also components of a second-rank tensor from the quotient law discussed in Section 1.5.4. Comparing (2.8) with (1.80), we infer that ni is an arbitrary tensor (It is arbitrary, since we may choose the direction of (n) the inclined surface.) and tk is a tensor. Therefore, we conclude that σik is a tensor. The importance of (2.8) is that it relates the stress vector t(n) acting on a plane with unit normal n to the stress tensor σ in the material element. Knowing n and t(n) , σ may be found from the equation. The stress tensor is expressed using the tensor bases as σ = σij ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

(2.10)

Stress

49 x2 22 21

23

12

32 11 31

13

x1

33

x3 FIGURE 2.3 Stress tensor components.

and in the symbolic notation, (2.8) is written as t(n) = σT · n

(2.11)

We now discuss the meaning of the stress components σij . These are intensity of forces (force per unit area) along the coordinate directions. They vary with the location in the body and their magnitudes and speciﬁc characteristics depend on the geometrical shape of the body and the loading condition (surface traction). To determine the distribution of stress in the body, we need to solve a boundary-value problem, by specifying the boundary conditions. However, this problem will not be discussed in this chapter. Instead, we concentrate on understanding the nature of stress at a given point, and consider the stress at a point. To visualize the stress at a point, we consider a parallelepiped cut out from the body. The size of the parallelepiped is not important as long as it is inﬁnitesimal. This is so, because, in the sense of calculus, we consider the stress at a point by taking the limit with the size of the parallelepiped of approaching zero. Figure 2.3 shows the components σij applied on the faces of the parallelepiped. The ﬁrst subscript denotes the direction of the normal to the considered plane and the second subscript denotes the direction in which the stress component acts. σ11 , σ22 , σ33 are the normal stresses and σ12 , σ21 , σ23 , σ32 , σ13 , σ31 are the shear stresses. For given n and t(n) on an inclined plane, show by coordinate transformation that σij are components of a tensor. With the orientation of the inclined surface ﬁxed, let us vary the choice of the coordinate system, so that we have xi and xi coordinate systems. In this exercise, n and t(n) remain ﬁxed. Using (2.6) and referring to the two coordinate

EXAMPLE 2.1

© 2005 by Chapman & Hall/CRC Press

50

Continuum Mechanics and Plasticity

systems, we have ti ni = t(n) = ti n i

(a)

Referring ti to the xi axes and ti to the xi axes, we write σij ej ni = σik e k n i

(b)

But, from (1.28) and (1.32), ej = Qjk e k

ni = Qip n p

and

(c)

So, by substitution σij Qjk e k Qip n p = σik e k n i

or

σij Qjk Qip n p = σik n i

(d)

Since this relation is true for all n, the above equation reduces to σij = Qki Qmj σkm

[σ ] = [Q]T [σ ][Q]

or

(e)

Therefore, we can conclude that σij are components of a second-rank tensor because they obey the transformation rule of a second-rank tensor. EXAMPLE 2.2

Show that the components of tensor equation (2.11) is (2.8). (n)

LHS of (2.11) = ti ei

(a)

RHS of (2.11) = σji ei ⊗ ej · nk ek = σji nk ei δlk = σji nj ei

(b)

Equating (a) with (b), we obtain (2.8).

2.5

Equations of Equilibrium

We derive the equations of equilibrium by summing all the forces applied to a body and reducing it to the local form. Refer to the body of Figure 2.1, and note that every portion of this body is in equilibrium. Consider that only surface tractions and body force apply to this body. The “global form” of the equations of equilibrium is then

V

© 2005 by Chapman & Hall/CRC Press

ρbi dV +

(n)

S

ti

dS = 0

(2.12)

Stress

51

By use of (2.8), (2.12) becomes

V

ρbi dV +

S

σji nj dS = 0

(2.13)

We now use the Gauss theorem to change the second integral of (2.13) into a volume integral. Then, we obtain V

(ρbi + σji,j ) dV = 0

(2.14)

Since the region of integration V is arbitrary and every part of the medium is in equilibrium, we conclude that the integrand must be zero to make the integral zero. Thus, ρbi + σji,j = 0

or

∂σji + ρbi = 0 ∂xj

(2.15)

Equations (2.15) are the equations of equilibrium in the local form, and they may be expanded into a familiar form as ∂σ21 ∂σ31 ∂σ11 + + + ρb1 = 0 ∂x1 ∂x2 ∂x3 ∂σ12 ∂σ22 ∂σ32 + + + ρb2 = 0 ∂x1 ∂x2 ∂x3

(2.16)

∂σ13 ∂σ23 ∂σ33 + + + ρb3 = 0 ∂x1 ∂x2 ∂x3 Show that the mean value theorem may be used to reduce the “global form” of the equations of equilibrium to the “local form.” The mean value theorem is

EXAMPLE 2.3

b a

f (x) dx = (b − a)f (ξ ),

with a ≤ ξ ≤ b

(a)

On the right-hand side of (a), the function f (ξ ) is evaluated at some point in the range of a and b. In the case of equation (2.14), the function f is ρbi + σji,j , which is evaluated at some interior point in V. Thus, (2.14) becomes V

(ρbi + σji,j ) dV = V(ρbi + σji,j ) = 0

(b)

Since V = 0, we obtain ρbi + σji,j = 0

© 2005 by Chapman & Hall/CRC Press

(c)

52

2.6

Continuum Mechanics and Plasticity

Symmetry of the Stress Tensor

The stress tensor is symmetric, that is, σ12 = σ21 , σ23 = σ32 , and σ31 = σ13 , so that the nine components of σij reduce to six independent components. This is not an assumption, but is the result of conservation of angular momentum. A simple way to show this is to project the stresses on the parallelepiped of Figure 2.3 onto a coordinate plane, say the (x1 − x2 ) plane, as shown in Figure 2.4. By summing moment about O, we get σ12 = σ21

(2.17a)

Similarly, by projecting the stresses and the parallelepiped onto the other two coordinate planes and summing moments about O, we ﬁnd σ23 = σ32

and

σ31 = σ13

(2.17b)

A rigorous proof of the symmetry of the stress tensor may be obtained by considering the conservation of angular momentum. We consider the general case that the body moment per unit volume Mi is included in the derivation. The effect of Mi will then be discussed. Referring to Figure 2.1, we have ρ(r × b)i = ρeijk xj bk = moment of ρbk about the origin (n)

(n)

(r × t(n) )i = eijk xj tk = moment of tk about the origin

(2.18) (2.19)

Summing moment about the origin O, we write V

ρeijk xj bk dV +

S

(n) eijk xj tk dS +

V

Mi dV = 0

x2 22 21 12 11

11 12 Ο

x1

21 22

FIGURE 2.4 2 D stress components.

© 2005 by Chapman & Hall/CRC Press

(2.20)

Stress

53

The second integral in (2.20) may be transformed into a volume integral by use of the Gauss theorem. Thus, (2.20) becomes ∂ ρeijk xj bk + (2.21) (eijk xj σrk ) + Mi dV = 0 ∂xr V The second term in (2.21) is ∂xj ∂σrk = eijk (σjk + xj σrk,r ) = eijk σjk + eijk xj (−ρbk ) σrk + xj eijk ∂xr ∂xr (2.22) where the last expression was obtained from the equations of equilibrium. Hence, (2.21) becomes [ρeijk xj bk + eijk σjk − ρeijk xj bk + Mi ] dV = 0 (2.23) V

which leads to V

(eijk σjk + Mi ) dV = 0

(2.24)

Since the integrand is continuous and the volume V is arbitrary, we obtain eijk σjk + Mi = 0

(2.25)

We now discuss the meaning of (2.25) in two different cases as follows: 1. If the body moment is absent, that is, Mi = 0, then (2.25) reduces to eijk σjk = 0

(2.26)

For i = 1, (2.26) gives e123 σ23 +e132 σ32 = 0. Since e123 = 1 and e132 = −1, we obtain σ23 = σ32 . For i = 2, (2.26) leads to σ13 = σ31 ; and for i = 3, (2.26) leads to σ21 = σ12 . Therefore, we write σij = σji

(2.27)

2. If Mi = 0, then σij = σji , and the stress tensor is not symmetric.

2.7

Principal Stresses

If we pass a plane through the parallelepiped of Figure 2.3 and cut the element into two parts, then one of the two parts may be viewed as a tetrahedron

© 2005 by Chapman & Hall/CRC Press

54

Continuum Mechanics and Plasticity x3

t ( n) n x2

O

x1

FIGURE 2.5 Stress vector on an inclined plane.

shown in Figure 2.5. Within the tetrahedron the stress is σij as deﬁned in Figure 2.3. The unit normal to the plane is n, and the associated stress vector t(n) may be found from (2.8) or (2.11). Generally, the two vectors n and t(n) have different directions as shown in Figure 2.5. We now inquire whether we can cut the parallelepiped in a speciﬁc direction (ﬁnd an n), such that n and t(n) have the same direction. If such an n exists, then t(n) = λn, where λ is the magnitude of vector t(n) . In this event, using (2.6), we obtain ti ni = λn

(2.28)

Substituting (2.7) into (2.28), we have σij ej ni = λnj ej

and

σij ni = λnj

(2.29)

which may be written as (σij − λδij )ni = 0

(2.30)

The solution of this set of equations would make t(n) lie in the direction of n. The solution includes ﬁnding the direction n and the magnitude λ. Mathematically speaking, (2.30) is a statement of the eigenvalue problem. The trivial solution ni = 0 of the homogeneous equations (2.30) does not satisfy the unit vector condition n21 + n22 + n23 = 1, so it cannot be our answer.

© 2005 by Chapman & Hall/CRC Press

Stress

55

The condition that a nontrivial solution exists for ni is that σ11 − λ |σij − λδij | = σ21 σ31

σ13 σ23 = 0 σ33 − λ

σ12 σ22 − λ σ32

(2.31)

Expanding the determinant in (2.31), we obtain λ3 − J1 λ2 + J2 λ − J3 = 0

(2.32)

where J1 = tr(σij ) = σii

σ J2 = tr cofactor(σij ) = 22 σ32

σ23 σ11 + σ33 σ31

σ13 σ11 + σ33 σ21

σ12 σ22

(2.33)

J3 = det σij The quantities J1 , J2 , and J3 are called the principal invariants of σij , because they remain invariant with a rotation of the coordinate system. Referring to two coordinate systems xi and xi , the invariants transform as σii = σii ,

tr cofactor(σij ) = tr cofactor(σij ),

det σij = det σij

(2.34)

Therefore, J1 = J1 , J2 = J2 and J3 = J3 . The stress invariants are further discussed in Section 2.11. Note that stresses (λ1 , λ2 , λ3 ) found by solving the characteristic equation (2.32) are called principal stresses and are often denoted by (σ1 , σ2 , σ3 ). In the mathematical language, λr (r = 1, 2, 3) are (r) eigenvalues and the three corresponding ni are eigenvectors. The eigenvalue problem is discussed in Section 2.8.

2.8

Properties of Eigenvalues and Eigenvectors

The eigenvalue problem is governed by equation (2.30). It is the governing equation of many engineering problems. The properties of the eigenvalues and eigenvectors for a symmetric tensor σij are summarized below: 1. Eigenvalues are real. 2. Eigenvectors are real. 3. Eigenvectors are orthogonal. 4. If eigenvalues are distinct, eigenvectors can be determined uniquely.

© 2005 by Chapman & Hall/CRC Press

56

Continuum Mechanics and Plasticity 5. If two eigenvalues are identical, one eigenvector corresponding to the distinct eigenvalue is unique, other two eigenvectors lie in a plane normal to the unique eigenvector. 6. If all three eigenvalues are identical, then all directions in the space xi are eigen directions. In this case σij = λδij . 7. The principal stress components σ¯ ij and the stress components σij are related by [σ¯ ] = [Q]T [σ ][Q], where the transformation matrix [Q] is deﬁned by the eigenvectors (direction cosines between the eigenvectors and coordinate axes) and this subject is discussed in Section 2.12.

Show that if σij is symmetric, then three real roots λ1 , λ2 , λ3 exist in (2.30). This is proven by contradiction. First, we let λ be complex, that is, λ = α+iβ. For the sake of generality, let ni be complex too, that is, ni = µi + iξi . Then, α, β, µi , and ξi are real. By substitution, (2.30) becomes EXAMPLE 2.4

σij (µi + iξi ) − (α + iβ)(µj + iξj ) = 0

(a)

By equating real and imaginary parts in (a), we obtain σij µi = αµj − βξj σij ξi = βµj + αξj

(b)

Multiplying the ﬁrst equation of (b) by ξj and the second equation of (b) by µj and subtracting the two resulting equations, we get β(ξj ξj + µj µj ) = 0

(c)

Since the quantity within the parenthesis is nonnegative, we have β=0

(d)

Hence, all eigenvalues are real. EXAMPLE 2.5

Show that if σij is symmetric, then all eigenvectors of (2.30)

are real. Proof Equation (2.30) may be written as (σ11 − λ)n1 + σ21 n2 + σ31 n3 = 0 σ12 n1 + (σ22 − λ)n2 + σ32 n3 = 0 σ13 n1 + σ23 n2 + (σ33 − λ)n3 = 0

© 2005 by Chapman & Hall/CRC Press

(a)

Stress

57

Because the determinant of (a) is zero, the rank is at most two (the rank of a matrix is the dimension of the largest square submatrix with a nonvanishing determinant that is contained in the matrix); therefore, the three equations are linearly dependent and the third equation can be expressed in terms of the former two. If we delete the last equation, then the number of equation is less than the number of unknown. Hence, a real solution for n1 , n2 , and n3 always exists. If the 3 × 2 matrix has rank two, then we can solve for n1 and n2 (say) in terms of n3 , that is, n1 = N1 n3

and

n2 = N2 n3

(b)

where N1 and N2 are proportional factors determined by the two equations. But n is a unit vector and it must satisfy n21 + n22 + n23 = 1

(c)

Substituting (b) into (c), we obtain (N12 + N22 + 1)n23 = 1

(d)

which may be solved to yield n3 = (1 + N12 + N22 )−1/2

(d)

Expressions in (b) and (e) form the solution of (a). In this case, n can be found uniquely. If the rank is less than two, then n cannot be determined uniquely, the physical signiﬁcance being that there may exist more than one n such that t(n) = λn

(f)

An example is, when σ11 = σ22 , then n cannot be determined uniquely. EXAMPLE 2.6

Show that eigenvectors are mutually orthogonal.

Case 1: All λ’s are distinct (r)

In this case λ1 = λ2 = λ3 . Choose two such directions ni then (2.30) becomes (r)

(r)

(s)

(s)

σij ni − λr nj = 0 σij ni − λs nj = 0

© 2005 by Chapman & Hall/CRC Press

(s)

and ni , r = s,

(a) (b)

58

Continuum Mechanics and Plasticity (s)

Multiplying (a) by nj equations, we ﬁnd

(r)

and (b) by nj , and subtracting the two resulting (r) (s)

(λr − λs )ni ni = 0 (r)

(c)

(s)

But since λr = λs , it follows that ni ni = 0, or n(r) · n(s) = 0, for r = s. Therefore, n(r) and n(s) are mutually orthogonal. In general, we may write (r) (s)

ni ni = δrs

(d)

Case 2: Two λ’s are not distinct Assume that λ1 = λ2 and λ2 = λ3 . Choose one characteristic direction n(1) and let x1 coincide with n(1) then σij will have the form

σ11

0 0

0 σ22

σ32

0

σ23

(e)

σ33

We then examine the characteristic direction in the xi system. The characteristic equation is (for λ = λ2 )

−λ σ11 2

0 0

T (2) n1 =0 σ23 n(2) 2 (2) σ33 − λ2 n3

0

0

−λ σ22 2 σ32

(f)

(2) (2) Evidently, n1 = 0, since the ﬁrst equation of (f) is σ11 − λ2 n1 = 0 and = λ = λ . This implies that x ⊥ n(2) or n(1) ⊥ n(2) . The remaining two σ11 1 2 1 equations are (2)

(2)

(σ22 − λ2 )n2 + σ23 n3 = 0 (2)

(g)

(2)

− λ2 )n3 = 0 σ32 n2 + (σ33 (2)

(2)

The determinant of (g) vanishes for nontrivial solution of n2 and n3 . Thus, (σ − λ2 ) σ23 =0 22 σ (σ33 − λ2 ) 32

(h)

or λ22 − λ2 (σ22 + σ33 ) − σ23 σ32 + σ22 σ33 = 0

© 2005 by Chapman & Hall/CRC Press

(i)

Stress

59

The two roots are + σ σ22 1 33 )2 − 4(σ σ − σ σ ) (σ22 + σ33 ± 22 33 32 23 2 2

σ + σ33 1 − σ )2 + 4(σ σ ) (σ22 ± = 22 33 32 23 2 2

λ2,3 =

(j)

The only condition which makes λ2 and λ3 not be distinct is for the discriminant to vanish, that is, = σ32 =0 σ23

and

σ22 = σ33 = λ2

(k) (2)

(2)

Substituting these results in (g), we see that any values of n2 and n3 and, (3) (3) similarly n2 and n3 , will satisfy the characteristic equation.

2.9

Normal and Shear Components

We observed in Section 2.7 that on an inclined plane with unit normal n, the stress vector t(n) and n generally have different directions. The two vectors have the same direction only when n is the principal direction of σij . In the general case, t(n) may be decomposed into two components: one in the normal direction denoted by σ N and the other in the tangential direction denoted by σ S as shown in Figure 2.6. σ N is called the normal component and σ S the shear component of the stress vector. The normal component is expressed by σ N = t(n) · n = σji nj ni

(2.35)

and the shear component is obtained from

N

|t(n) |2 = (σ N )2 + (σ S )2

n S

FIGURE 2.6 Normal and shear stress components.

© 2005 by Chapman & Hall/CRC Press

t (n)

(2.36)

60 2.9.1

Continuum Mechanics and Plasticity Directions Along which Normal Components of σij are Maximized or Minimized

We like to ﬁnd an n such that σ N is maximized or minimized. It is noted that n is subject to the condition ni ni = 1. The method of Lagrangian multiplier denoted by λ is used, so that we maximize or minimize the expression F = σji ni nj − λni ni

(2.37)

The differentiation of (2.37) yields ∂F =0 ∂ni

or

σji nj − λni = 0

(2.38)

But, (2.38) is the condition that ni be a principal direction. Hence, the principal directions make σ N either maximum or minimum, and the max. (or min.) normal component is equal to the max. (or min.) principal value of σij .

2.9.2

The Maximum Shear Stress

We use (2.36) to obtain the expression of the shear component σ S . We ﬁnd ﬁrst from (2.8) and (2.35) the following expressions: |t(n) |2 = σji nj σki nk

(2.39)

(σ N )2 = σji ni nj σmk nk nm

(2.40)

For simplicity, we let xi coincide with principal axes, then we have only the principal stresses σ1 , σ2 , σ3 and the shear stresses are zero. In this case, (2.35) reduces to σ N = σ1 n21 + σ2 n22 + σ3 n23

(2.41)

|t(n) |2 = σ12 n21 + σ22 n22 + σ32 n23

(2.42)

and (2.39) becomes

Substituting (2.41) and (2.42) into (2.36), we obtain 2 (σ S )2 = σ12 n21 + σ22 n22 + σ32 n23 − σ1 n21 + σ2 n22 + σ3 n23

(2.43)

or (σ S )2 + [(σ1 n21 ) + (σ2 n22 ) + σ3 (1 − n21 − n22 )]2 = σ12 n21 + σ22 n22 + σ32 (1 − n21 − n22 ) (2.44)

© 2005 by Chapman & Hall/CRC Press

Stress

61

To ﬁnd the maximum σ S , we set the derivatives to zero: ∂(σ S )2 = 0, ∂n1

∂(σ S )2 =0 ∂n2

(2.45)

and we ﬁnd 2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n1 (σ1 − σ3 ) = n1 (σ12 − σ32 )

(2.46)

2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n2 (σ2 − σ3 ) = n2 (σ22 − σ32 )

(2.47)

We now discuss three cases depending on whether the principal stresses are distinct or not. Case 1:

The three principal stresses are distinct, that is, σ1 = σ2 = σ3

Common factors of (σ1 − σ3 ) and (σ2 − σ3 ) can be cancelled out from (2.46) and (2.47), respectively, so that the two equations become 2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n1 = n1 (σ1 + σ3 )

(2.48)

2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n2 = n2 (σ2 + σ3 )

(2.49)

It follows that n1 and n2 cannot both be different from zero, because otherwise n1 can be cancelled out from (2.48) and n2 cancelled out from (2.49) to obtain the following two equations: σ 1 + σ3 =0 2

σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 ) −

(2.50)

σ 2 + σ3 =0 (2.51) 2 If these two equations are to be satisﬁed, we must have σ1 = σ2 , in contradiction with the hypothesis that σ1 = σ2 . Either n1 or n2 , therefore, must be zero. Let n1 = 0, then from (2.49) we obtain σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 ) −

2[σ2 n22 + σ3 (1 − n22 )]n2 = n2 (σ2 + σ3 )

(2.52)

which may be simpliﬁed to n22 (σ2

σ2 − σ3 − σ3 ) = 2

or

n2 = ±

1 = ± cos 45◦ 2

(2.53)

Therefore, the solution is

n1 = 0,

© 2005 by Chapman & Hall/CRC Press

1 , n2 = ± 2

n3 = ±

1 2

(2.54a)

62

Continuum Mechanics and Plasticity n

x2

45°

x3

x1

n3 = 0 n3 = 0 S

x2

S

S

n1 = 0 n2 = 0 x1 FIGURE 2.7 Maximum shear stresses.

The other two cases are

1 n1 = ± , 2 1 n1 = ± , 2

n2 = 0,

1 2

(2.54b)

n3 = 0

(2.54c)

n3 = ±

n2 = ±

1 , 2

The shear stresses σ S active in the planes of n1 = 0, n2 = 0, or n3 = 0 are shown in Figure 2.7. In the insert, we show the plane of n3 = 0. It is seen that the maximum shear stresses are making ±45◦ angles with the coordinate axes. Finally, we note that in all cases of (2.54) σS =

σ2 − σ3 2

or

σ 1 − σ3 2

or

σ 1 − σ2 2

(2.55)

which may be obtained by substituting, respectively, the planes of (2.54a,b,c) into equation (2.44) for σ S . Case 2: Two principal stresses are not distinct and we consider the case of σ2 = σ3 = σ1

© 2005 by Chapman & Hall/CRC Press

Stress

63

O

45°

x1

45°

FIGURE 2.8 Maximum shear stress in the case of σ2 = σ3 = σ1 .

This is a case of rotational symmetry about the x1 -axis. In this case, n2 is arbitrary; since σ3 = σ1 , we may use (2.48) to obtain n21 (σ1 − σ3 ) =

σ1 − σ3 2

(2.56)

We note that n1 = 0, because, if n1 = 0, then upon choosing n2 = 0, we obtain n3 = 1. Using (2.44), the case of n1 = 0 leads to σ S = 0, which is the minimum shear stress, in contradiction with the goal of ﬁnding the maximum shear stress. Simplifying (2.56), we ﬁnd n1 = ±

1 , 2

n2 = arbitrary,

n3 = arbitrary

(2.57)

In this discussion, special attention is given to the relation n21 + n22 + n23 = 1. Figure 2.8 shows a cone with generator in the x1 direction. The maximum shear stress σ S lies on the surface of the cone and its magnitude is given by σ S = 12 (σ1 − σ2 ) found on substitution of (2.57) into (2.44). Case 3: All principal stresses are equal, that is, σ1 = σ2 = σ3 = σ This is a case of hydrostatic pressure. In this case, we found from (2.43) that (σ S )2 = σ 2 (n21 + n22 + n23 ) − σ 2 (n21 + n22 + n23 )2 = 0

(2.58)

with arbitrary n1 , n2 , n3 , that is, the shear stress is zero in all directions. Finally, the following conclusion may be stated: the maximum shear stress is equal to one-half the difference between the greatest and least normal stresses and acts on the plane that bisects the angle between the directions of the largest and smallest principal stresses.

© 2005 by Chapman & Hall/CRC Press

64

2.10

Continuum Mechanics and Plasticity

Mean and Deviatoric Stresses

Any tensor of rank two can be written as (C11 + C22 + C33 ) δij Cij = αδij + Bij = 3 C13 C12 {C11 − 13 (C11 +C22 + C33 )} 1 C21 {C22 − 3 (C11 C23 + +C22 + C33 )} 1 C31 C32 {C33 − 3 (C11 +C22 + C33 )}

(2.59)

In a similar manner, the stress tensor σij can be written as σij =

(σ11 + σ22 + σ33 ) δij 3 σ13 σ12 {σ11 − 13 (σ11 +σ22 + σ33 )} σ21 {σ22 − 13 (σ11 σ23 + +σ22 + σ33 )} 1 σ31 σ32 {σ33 − 3 (σ11 +σ22 + σ33 )}

(2.60)

or σij = 13 σkk δij + σij

(2.61)

where 13 σkk is the mean stress; and σ13 σ12 {σ11 − 13 (σ11 +σ22 + σ33 )} 1 σ21 σ23 {σ22 − 3 (σ11 σij = +σ22 + σ33 )} σ31 σ32 {σ33 − 13 (σ11 +σ22 + σ33 )}

(2.62)

is the deviatoric stress tensor. Thus, the stress may be decomposed into the hydrostatic (mean stress) and deviatoric parts. This property of stress is particularly useful in the study of plasticity which is discussed further in the later chapters of this book. Plastic yielding and plastic deformation of metals are known to be independent of the hydrostatic stress but are dependent on the deviatoric stress. © 2005 by Chapman & Hall/CRC Press

Stress

2.11

65

Octahedral Shearing Stress

The concept of octahedral shearing stress is useful in plasticity as well. Consider principal stress axes. If the normal ni of a plane in this stress space makes equal angles with the three axes, there are eight directions which satisfy n21 = n22 = n23 = 13 . The eight planes associated with these eight directions are called the octahedral planes. The planes form equal angles with the principal directions and form a diamond shaped region around the zero stress point. The shearing stress σoS that acts on the octahedral planes is called the octahedral shearing stress. From (2.43), in the principal stress space, we can show that the align reduces to (σ S )2 = (σ1 − σ2 )2 n21 n22 + (σ2 − σ3 )2 n22 n23 + (σ3 − σ1 )2 n23 n21

(2.63)

If n21 = n22 = n23 = 13 , then (2.63) reduces to 9(σoS )2 = (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2

(2.64)

This is the expression for octahedral shearing stress. On the other hand, the normal component acting on the octahedral plane is given from (2.41) by σoN = 13 (σ1 + σ2 + σ3 ) = mean stress

(2.65)

We now show that the octahedral shearing stress may be expressed in terms of the stress invariants. To this end, we observe that align (2.64) can be rewritten as: 9(σoS )2 = 2(σ12 + σ22 + σ32 ) − 2(σ1 σ2 + σ2 σ3 + σ3 σ1 ) = 2[(σ1 + σ2 + σ3 )2 − 2(σ1 σ2 + σ1 σ3 + σ2 σ3 )] − 2(σ1 σ2 + σ2 σ3 + σ3 σ1 ) = 2[J12 − 2J2 ] − 2J2 = 2J12 − 6J2

(2.66)

where (2.33) was used in the principal coordinate system. It is seen that the octahedral shearing stress σoS is invariant with rotation of coordinate axes. If J1 and J2 are expressed in terms of stress components taken relative to arbitrary (x1 , x2 , x3 ) axes — not principal axes as above —, equation (2.66), on the substitution of (2.33), becomes 2 2 2 + 6σ13 + 6σ23 9(σoS )2 = (σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 + 6σ12 (2.67)

This expression forms the basis for von Mises yield criterion discussed in Chapter 6 . © 2005 by Chapman & Hall/CRC Press

66

2.12

Continuum Mechanics and Plasticity

The Stress Invariants

We would like to see now that the stress invariants deﬁned in (2.33) remain unchanged under rotation of the coordinate system. Let us assume that coordinates xi rotate into xi . The ﬁrst stress invariant is J1 = σii

(2.68)

In the coordinate system xi , we denote the components of σij by σij , then the ﬁrst invariant in the xi system is J1 = σii . Using the transformation align of the second-rank tensor (1.46), we have σii = Qri Qsi σrs = δrs σrs = σss = σii

(2.69)

Comparing (2.68) and (2.69), we ﬁnd J1 = J1

(2.70)

which shows that J1 indeed remains unchanged with rotation of the coordinate system. The third invariant is J3 = det σ = 16 eijk erst σir σjs σkt

(2.71)

In the primed coordinate system, J3 = 16 eijk erst σir σjs σkt = 16 eijk erst Qai Qbr σab Qcj Qds σcd Qek Qft σef = 16 (eijk Qai Qcj Qek )(erst Qbr Qds Qft )σab σcd σef = 16 eace ebdf σab σcd σef = J3

(2.72)

It is seen from (2.72) that J3 is an invariant. In the derivation of (2.72), we = e , which indicates that the permutation symbol is a used the relation eijk ijk third-rank isotropic tensor. The second invariant is J2 = tr cofactor σ = Mii

(2.73)

Note that we use Mij to denote the matrix of the cofactors and not the minors. We now ﬁnd the expressions for the minors. To do this, we ﬁrst expand the

© 2005 by Chapman & Hall/CRC Press

Stress

67

determinant of the stress matrix as σ11 σ12 σ13 σ21 σ22 σ23 = σ11 σ22 σ23 − σ12 σ21 σ32 σ33 σ31 σ31 σ32 σ33

σ21 σ23 + σ 13 σ33 σ31

σ22 σ32

(2.74)

We then differentiate (2.74) to obtain the minors as M11 =

∂|σ| , etc. ∂σ11

(2.75)

∂|σ| ∂σij

(2.76)

Generally, we write Mij =

Using (2.76) and (2.71), and observing the notations ∂σir = δip δrq ∂σpq

(2.77)

Mpq = 16 {epjk eqst σjs σkt + eipk erqt σir σkt + eijp ersq σir σjs }

(2.78)

We ﬁnd

The second and third terms on the right-hand side are equal to the ﬁrst term, and (2.78) may be simpliﬁed to obtain Mpq = 21 epjk eqst σjs σkt

(2.79)

Hence, we ﬁnd J2 = Mii = 12 eijk eist σjs σkt = 12 (δjs δkt − δjt δks )σjs σkt = 12 {σjj σkk − σjk σkj } = 12 {[tr σ]2 − tr(σ)2 } = 12 {J12 − tr(σ2 )}

(2.80)

Since J1 and tr(σ2 ) are invariant, we may conclude that J2 remains invariant with rotation of the coordinate system. Another representation of J2 may be obtained as follows. Using (2.79), we write Mpq σrq = 12 epjk eqst σjs σkt σrq

(2.81)

By use of the identity proven in Example 2.7, (2.81) reduces to σrq Mpq = 12 epjk erjk |σ| = δpr |σ|

© 2005 by Chapman & Hall/CRC Press

(2.82)

68

Continuum Mechanics and Plasticity

Note that the identity eirs ejrs = 2δij has been used in the derivation of (2.82). In the symbolic notation, (2.82) may be written as σ · MT = 1 · |σ|

(2.83)

If we multiply (2.83) from the left by σ−1 , we obtain MT = σ−1 |σ|

or

σ−1 =

MT |σ|

(2.84)

This indicates that the inverse of the matrix σ is the transpose of its cofactors divided by the determinant of the matrix. Using (2.84), we ﬁnd the following expression for the second invariant J2 = tr(M) = tr MT = tr(σ−1 )|σ| EXAMPLE 2.7

(2.85)

Prove the identity empq det A = eijk Aim Ajp Akq .

Proof The determinant of matrix [A] is A11 det A = A21 A31

A12 A22 A32

A13 A11 A23 = A12 A33 A13

A21 A22 A23

A31 A32 A33

(a)

An interchange of column or row of the determinant causes a sign change, and this may be expressed by A1m empq det A = A2m A3m

A1p A2p A3p

A1q A1m A2q = A1p A3q A1q

A2m A2p A2q

A3m A3p A3q

(b)

A triple product of three vectors is a1 a · (b × c) = eijk ai bj ck = b1 c1

a2 b2 c2

a3 b3 c3

(c)

When we let ai = Aim , bi = Aip , and ci = Aiq , (b) and (c) combine to give empq det A = eijk Aim Ajp Akq

© 2005 by Chapman & Hall/CRC Press

(d)

Stress

69

which proves the identity. Finally, we note that i a × b = ax b x

2.13

j ay by

k i az = j bz k

ax ay az

bx by bz

(e)

Spectral Decomposition of a Symmetric Tensor of Rank Two

In this section, we discuss a representation of a symmetric second rank tensor by its eigenvalues and eigenvectors. To this end, we derive the following relation ﬁrst (r) (r)

ni nj = δij

(r summed)

(2.86) (1)

(2)

(3)

If we denote the directions of the normalized eigenvectors ni , ni , ni by x1 , x2 , x3 , respectively, we can then make use of (1.22), which relates the base vectors of the two coordinate systems. Thus, unit vectors n(r) may be represented by (r)

n(r) = nk ek = Qkr ek

(2.87)

(r)

where nk are direction cosines of n(r) with respect to the ek system and (r)

nk = Qkr

(2.88)

The inverse of (2.87) is (r)

ek = nk n(r)

(2.89)

On the other hand, following the same procedure and using a different normalized eigenvector, we obtain (s) em = n(s) m n

(2.90)

We then form the dot product from (2.89) and (2.90) as, (r)

(r)

(r)

(s) (r) ek · em = nk n(r) · n(s) = nk n(s) m n m δrs = nk nm

(2.91)

In the derivation, we note that eigenvectors are orthogonal expressed by (r) (s)

ni ni = δrs

© 2005 by Chapman & Hall/CRC Press

(2.92)

70

Continuum Mechanics and Plasticity

Hence (2.91) reduces to (r)

nk n(r) m = δkm

(2.86)

We now use this result to derive a representation of a symmetric tensor by its eigenvalues and eigenvectors. To this end, we start with (r)

(r)

σij ni = λr nj

(r not summed)

(2.93)

(r)

Then, by multiplying both sides of (2.93) by nk and summing over r, we have (r) (r)

σij ni nk =

(r) (r)

λ r nj nk

(2.94)

r

Using (2.86), (2.94) reduces to σij =

(r) (r)

λ r ni nj

(2.95)

r

Equation (2.95) is the spectral decomposition of σij . A remark is in order. In the study of coordinate transformation in Chapter 1, we have Qki Qkj = δij

(1.25)

Qik Qjk = δij

(1.27)

where Qij is the transformation matrix between coordinate systems xi and xi . In this section, we obtain the relations (r) (s)

ni ni = δrs

(2.92)

(r) (r)

ni nj = δij

(2.86)

(r)

(r)

where ni are normalized eigenvectors. Since from (2.88) nk = Qkr , then upon substitution, (2.92) and (2.86) reduce to (1.25) and (1.27), respectively. Also, the [Q] matrix may be written as

(1)

n1

[Q] = [n(1)

n(2)

(1) n(3) ] = n2 (1)

n3

© 2005 by Chapman & Hall/CRC Press

(2)

n1

(2)

n2

(2)

n3

(3)

n1

(3) n2 (3) n3

(2.96)

Stress

2.14

71

Powers of a Tensor

Powers of a tensor σij is usually written as Square of σij = σip σpj = σ2

(2.97)

Cube of σij = σip σpq σqj = σ3 , etc.

(2.98)

For a second-rank symmetric tensor, we have the representation σij =

(r) (r)

λr ni nj

(2.99)

r

If n is a positive integer, the nth power of a tensor σ deﬁned to be the positive tensor σn whose components are σijn =

(r) (r)

λnr ni nj

(2.100)

r

This expression may be proven as follows: from (2.30), we have σij ni = λnj , so that (σij σjp )ni = λσjp nj = λ2 np

(2.101)

which shows that the square of σij has the eigenvalue of λ2 and the eigenvector of ni . The same method may continue for the third power of σij and for the general case of nth power. If n is a fraction number, then all eigenvalues need be positive. A tensor σ is said to be positive, if it has positive principal values and three linearly independent principal vectors (eigenvectors). A tensor σ is said to be positive deﬁnite if it is coefﬁcients of a positive deﬁnite quadratic form. It may be easily shown that a positive symmetric tensor is also positive deﬁnite.√Knowing a positive σ, we can ﬁnd the square root of this tensor σ1/2 = σ by ﬁrst ﬁnding the principal directions and the principal values σ1 , σ2 , and σ3 of σ; and then, in the principal space, we take the square root of the principal values so that the matrix is 1/2 σ1 0 0 1/2 σ¯ 1/2 = 0 (2.102) 0 σ2 1/2 0 0 σ3 Finally, we apply the transformation equation to obtain σ1/2 referred to the xi axes. The equation used in the axes transformation is [σ ]1/2 = [Q][σ¯ ]1/2 [Q]T

© 2005 by Chapman & Hall/CRC Press

(2.103)

72

Continuum Mechanics and Plasticity

Show that a positive symmetric tensor is also positive deﬁnite. If a tensor is positive, its eigenvalues are all positive, that is, λ1 > 0, λ2 > 0, λ3 > 0. In the principal coordinate system, the expression of quadratic form σij ni nj is λ1 n21 + λ2 n22 + λ3 n23 . If λ1 > 0, λ2 > 0, and λ3 > 0, then λ1 n21 + λ2 n22 + λ3 n23 > 0, which shows that the quadratic form is positive deﬁnite. On the other hand, it may be shown that a positive deﬁnite (symmetric) tensor is positive. To this end, we consider σij ni nj > 0. In the principal coordinate system, the quadratic form is reduced to

EXAMPLE 2.8

λ1 n21 + λ2 n22 + λ3 n23 > 0

(a)

We note that ni is one of the eigenvectors, so that if n1 = 0 and n2 = n3 = 0, (a) reduces to λ1 n21 > 0, which leads to λ1 > 0. Similarly, λ2 > 0, λ3 > 0 and, therefore, σ is a positive tensor.

2.15

Cayley–Hamilton Theorem

The aim of this section is to indicate that, by use of the Cayley–Hamilton theorem, a high-order matrix polynomial may be reduced to a lower order one. In this manner, a nonlinear expression can be reduced to an expression with second-order term as its highest power term, and thus simplifying the mathematics involved. According to this theorem, a square matrix satisﬁes its own characteristic align, that is, σ3 − J1 σ2 + J2 σ − J3 δ = 0

(2.104)

In the principal space, (2.104) is written as λ3r − J1 λ2r + J2 λr − J3 = 0

where r = 1, 2, 3

(2.105)

and, in the matrix form, (2.105) is

σ13 0 0

0 σ23 0

2 0 σ1 0 − J1 0 σ33 0

0 σ22 0

0 σ1 0 + J2 0 0 σ32

0 σ2 0

0 1 0 − J3 0 σ3 0

0 1 0

0 0 = 0 1 (2.106)

where σ1 , σ2 , σ3 are the three principal values. In the index notation, (2.104) is written as σim σmn σnj − J1 σim σmj + J2 σij − J3 σij = 0

© 2005 by Chapman & Hall/CRC Press

(2.107)

Stress

73

This equation is valid in the general case and not necessarily in the principal directions. But the formal proof is lengthy and is to be found in a textbook on linear algebra. The proof will not be discussed here. We show next that the expression of J2 may be found by using this theorem. Multiplying (2.104) by σ−1 , we ﬁnd σ2 − J1 σ + J2 δJ3 σ−1 = 0

(2.108)

Taking the trace of all terms in the above equation, we obtain tr σ2 − J12 + 3J2 − J3 tr(σ−1 ) = 0

(2.109)

Since the last term is, from (2.85), −J2 , (2.109) may be solved to yield J2 = 12 (J12 − tr σ2 )

(2.110)

This expression is similar to that derived earlier in (2.80). By use of the Cayley–Hamilton theorem, we can reduce the nth (positive integer) power of a matrix to a linear combination of the second, ﬁrst, and zeroth powers. For example, if we multiply (2.104) by σ, we obtain σ 4 − J 1 σ3 + J 2 σ2 − J 3 σ = 0

(2.111)

By applying (2.104) again, (2.111) becomes σ4 − J1 {J1 σ2 − J2 σ + J3 δ} + J2 σ2 − J3 σ = 0

(2.112)

σ4 = σ2 {J12 − J2 } − σ{J1 J2 − J3 } + J1 J3 δ

(2.113)

which leads to

It is seen that σ4 may be expressed in terms of σ2 , σ, and δ. It is important to note that the coefﬁcients of the second, ﬁrst, and zeroth-power terms are functions of the invariants of σ. In a similar manner, a matrix of any power higher than two may be expressed in terms of σ2 , σ, and δ.

References 1. Malvern, L.E., Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Englewood Cliffs, NJ, 1969. 2. Prager, W., Introduction to Mechanics of Continua, Ginn, Boston, MA, 1961. 3. Eringen, A.C., Mechanics of Continua, Wiley, New York, 1967.

© 2005 by Chapman & Hall/CRC Press

74

Continuum Mechanics and Plasticity 4. Fung, Y.C., Foundations of Solid Mechanics, Prentice-Hall, Englewood Cliffs, NJ, 1965. 5. Truesdell, C. and Toupin, R., The Classical Field Theories, in Handbuch der Physik, Vol. III/1, S. Flugge, Ed., Springer-Verlag, Berlin, 1960. 6. Sokolnikoff, I.S., Mathematical Theory of Elasticity, McGraw-Hill, New York, 1956.

Problems (1) A specimen used for uniaxial tensile testing of material has a middle section (the gauge section) of reduced cross-section. The stress is uniformly distributed within this section. You may consider this section as a circular cylinder. When the specimen is pulled, what stress boundary conditions (stress vectors) apply in the middle section of the specimen? (2) An inﬁnitesimal material element is subjected to hydrostatic pressure p as shown in Figure 2.9. Determine the stress vector acting on surface a–a of the element.

p

a⬘ p

p a

p

FIGURE 2.9

(3) The bar shown in Figure 2.10 has a cross-sectional area A and is subjected to the axial load P. Determine the stress vector acting on the inclined surface a–a .

a⬘ P

P a

FIGURE 2.10

© 2005 by Chapman & Hall/CRC Press

Stress

75

(4) The state of stress for the inﬁnitesimal tetrahedron OABC shown in Figure 2.11 is

20 [σ ] = −60 40

−60 0 80

40 80 MPa −20

Determine the stress vector acting on the inclined plane ABC. x3

C(0,0,1)

B(0,1,0)

O

x2

A(2,0,0) x1 FIGURE 2.11

(5) Let the components of the stress tensor at point P be given in matrix form by

21 [σ ] = −63 42

−63 0 84

42 84 MPa −21

Determine the stress vector on a plane passing through P, parallel to the x3 -axis and making a 30◦ counterclockwise angle from the x1 -axis. (6) If the components of the stress tensor is given by

1 σij = 0.5 0

0.5 −1 −0.2

0 −0.2 MPa 0

determine √ the stress vector acting on a surface whose normal is n = 0.2e1 + 0.3e2 + 0.87e3 . What are the normal and shear components acting on the surface? (7) In the principal stress space, determine the expression of stress vector (in terms of stress components) acting on the octahedral plane in the ﬁrst quadrant of the stress space.

© 2005 by Chapman & Hall/CRC Press

76

Continuum Mechanics and Plasticity (8) Stress is a second-rank tensor. If the stress components referring to the xi coordinate system are

6 [σij ] = 2 0

2 −1 0

0 0 MPa 1

ﬁnd the stress components of the same tensor with respect to the xi system if x3 = x3 and x1 is making a 30◦ angle counterclockwise with the x1 -axis. (9) The stress tensor at point P has the following components with respect to the xi coordinate system

20 [σ ] = 0 −10

0 8 0

−10 0 MPa 24

Referring to Figure 2.12, if the x1 -axis makes equal angles θ with the three xi axes and the x2 -axis lies in the x1 x2 plane, determine the components of the stress tensor referred to the right-handed xi coordinate system. x3

x⬘1 P

x2

x1

x⬘2

FIGURE 2.12

(10) The stress tensor is σij = α(νi νj + νj νi ), where α is a scalar and ν and ν are unit vectors. Determine the principal stresses and axes. (Hint: to simplify the computation, choose the x1 -axis parallel to ν and the x3 -axis normal to ν and ν ).

© 2005 by Chapman & Hall/CRC Press

Stress

77

(11) Let t1 , t2 , and t3 be the stress vectors acting on surface elements that are normal to the coordinate axes. Show that the sum of the squares of the magnitudes of these vectors is independent of the orientation of the coordinate axes. (12) Consider the following stress distribution

ax2 σ= b 0

b 0 0

0 0 0

where a and b are constants. Determine and sketch the distribution of the stress vector acting on the square in the x1 = 0 plane, with vertices located at (0, 1, 1), (0, −1, 1), (0, 1, −1), (0, −1, −1). (13) A block of unit thickness is subjected to forces shown in Figure 2.13. The area of face (1) is A1 and the area of face (2) is A2 . (a) Determine the stress vectors acting on these two surfaces; (b) ﬁnd the conditions which must be satisﬁed by the forces and areas for the block to be in equilibrium; (c) if the stress is uniformly distributed in the block, determine the components of the stress tensor; (d) if principal stresses apply on the material element shown with orientation speciﬁed by φ, ﬁnd the second stress invariant J2 at this conﬁguration. x2 F4

Face 2

F3 F2 F1

x1

Face 1

FIGURE 2.13

(14) For the state of stress given by

10 [σ ] = 30 −50

30 0 0

−50 0 MPa 0

ﬁnd the components of the deviatoric stress σij and determine the principal invariants of the deviatoric stress.

© 2005 by Chapman & Hall/CRC Press

78

Continuum Mechanics and Plasticity

(15) Cut out a tetrahedron of inﬁnitesimal size from a body. The normal of the inclined face makes equal angles with the three coordinate axes. Find the force that must be applied on the inclined face so that it will produce a state of stress given by the following matrix

30 [σ ] = −10 20

−10 0 10

20 10 MPa 10

For equilibrium, what forces must be applied to the faces normal to the coordinate axes? (16) The second invariant of the deviatoric part of σ is denoted by J2 . Show that . Note that the differentiation is taken with respect to σ and ∂J2 /∂σpq = −σqp pq not σpq . (17) If [Q] = [n(1) n(2) n(3) ] and [Q]T [Q] = [δ], show that by use of (σij − λδij )ni = 0, it may be shown that

λ1 [Q]T [σ ][Q] = 0 0

0 λ2 0

0 0 λ3

that is, [σ ] may be diagonalized by use of [Q]. Show also that tr QT σQ = λ1 + λ2 + λ3 . (18) A stress ﬁeld is given by the matrix

(1 − x22 )x1

0

(1 − x22 )x1

− 12 (x22 − 4x2 )

0

0

0

(4 − x12 )x2

[σ ] =

(1 + x12 )x2 + 12 x22

Find the expression for the second invariant of the deviatoric stress. (19) If J1 , J2 , and J3 denote the principal invariants of the stress tensor σij and J1 , J2 , and J3 denote the principal invariants of the deviatoric stress σij , show that J1 = J1 + 3σm = 3σm 1 J2 = J2 + J12 3 2 1 3 J3 = J3 + J1 J2 + J 9 27 1

© 2005 by Chapman & Hall/CRC Press

3 Motion and Deformation

3.1

Introduction

In this chapter, we consider the motion of a body and, in particular, we concentrate on the study of deformation and the rate of change of a material element on or within the body. We assume the reader has familiarized himself with the concepts of strain and strain-rate in the study of elementary mechanics of deformable bodies. Strain describes the change in the geometry of an element in a body. But strain and strain-rate need to be deﬁned. There are several measures of strain that people use. Deformation is a more general terminology to use than strain in describing the geometrical change of a material element (see [1–4] for further reading). The particles of the body may occupy various positions in a threedimensional space. The complete speciﬁcation of the positions of the particles of a body is called the conﬁguration of a body. The conﬁguration of the body at the reference time (or initial or undeformed state) and at the current time (or deformed state) is the reference conﬁguration denoted by R0 , and the current conﬁguration denoted by Rt , respectively. To ﬁx the concept of deformation, let us consider a material point P within a neighborhood N0 at the reference conﬁguration. Referred to in Figure 3.1, point P moves to point p within a neighborhood Nt at the current conﬁguration due to load applied to the body. The concept of deformation may be understood by taking two photographs of the material element, one at the reference conﬁguration and the other at the current conﬁguration. We then compare and characterize the size and shape of the material element in the two photographs. The change in the size and shape of the material element is called the deformation of the material element and it indicates its need to be quantiﬁed. We also observe that time is not a factor in the study of deformation. To describe the two conﬁgurations, a material (Lagrangian) coordinate system, denoted by XR , and a spatial (Eulerian) coordinate system, denoted by xi , is introduced. The position of the material point P at the reference conﬁguration is speciﬁed by the material coordinates XR and that of p at the current conﬁguration is speciﬁed by the spatial coordinates xi . For convenience, the undeformed conﬁguration of a material element is often chosen as the 79

© 2005 by Chapman & Hall/CRC Press

80

Continuum Mechanics and Plasticity

p(xi) Nt

Rt

P(XR) N0

R0 x3

X3

eR

O

ei

x2

X2

O X1

x1

FIGURE 3.1 Reference and current conﬁgurations.

reference conﬁguration. But, any other conﬁguration may also be chosen as the reference conﬁguration, if needed. Once a reference conﬁguration has been chosen, all the material points of a body can be described by the material coordinates XR . In the general case, the axes of XR and xi do not have the same origin and orientation as shown in Figure 3.1. But, in many cases, it is convenient to select the two coordinate systems such that they have the same origin and orientation. This selection leads to simplicity and is used in most of the topics discussed in this book. Motion may be viewed as a family of deformations continuously varying in time, and the deformations between two conﬁgurations have been discussed in the previous paragraph. When a continuum is in motion, physical quantities associated with a material element of the body (such as density ρ, velocity v, etc.) change with location and time. The motion of a continuous body may be described in two ways: material and spatial descriptions. The material description has been used mostly in solid mechanics and the spatial description in ﬂuid mechanics. Some recent works have used a mixed description. We now discuss the two descriptions in the light of time-dependent motions.

3.2 3.2.1

Material and Spatial Descriptions Material Description

The material description is also known as the Lagrangian description. In this description, a material element is followed. The observer sits on top of the body and moves with the body. He observes changes in the physical

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

81

quantities of the body as functions of the material element identiﬁed by the material coordinates XR and time t. Therefore, we write ρ = ρ(XR , t),

3.2.2

v = v(XR , t), etc.

(3.1)

Spatial Description

The spatial description is also known as the Eulerian description. Here, the observer observes the changes in physical quantities at a ﬁxed location in the laboratory. Hence, the quantities are described in terms of the location in space denoted by the spatial coordinates xi and time t. In effect, we describe and measure the quantities at a ﬁxed location and they are functions of time. Spatial positions are occupied by different particles at different times. Therefore, the spatial description does not provide direct information related to changes in the properties of the material element as the body moves. In this description, we write ρ = ρ(xi , t),

v = v(xi , t), etc.

(3.2)

If we know the motion of the body, then the two descriptions are related and are equivalent. One description can be obtained from the other. The correlation between the two descriptions is now discussed. During the motion of the body, particle P with position vector X moves to point p with position vector x and the displacement is u=x−X

(3.3)

In the material description, the above equation is written as u(X, t) = x(X, t) − X

(3.4)

and, in the spatial description, it is written as u(x, t) = x − X(x, t)

(3.5)

The velocity v of a particle is the rate of change of its displacement, and, in the material description, it is written as v(X, t) =

∂[x(X, t) − X] ∂x(X, t) Dx ∂u(X, t) = = ≡ ∂t ∂t ∂t Dt

(3.6)

where D/Dt is called the material derivative. The motion of the particle is followed and material coordinate X is ﬁxed during this motion. In the index

© 2005 by Chapman & Hall/CRC Press

82

Continuum Mechanics and Plasticity

notation, (3.6) is written as vi (XR , t) =

∂xi (XR , t) ∂t

(3.7)

Note that the expression in (3.7) is different from the spatial description, which is vi (xj , t) for the particle velocity. The relationship between the two descriptions is illustrated in Example 3.1. EXAMPLE 3.1

A body undergoes the motion deﬁned by x1 = X1 (1 + a1 t + a2 t2 ),

x2 = X2 ,

x3 = X3

(a)

where a1 and a2 are constants. Find the displacement and velocity in both the material and spatial descriptions. Solution In the material description, we have from (3.4), ui (XR , t) = xi (XR , t) − Xi

(b)

When equation (a) is substituted into (b), we obtain u1 = x1 − X1 = X1 (a1 t + a2 t2 ) u2 = x2 − X2 = 0

(c)

u3 = x3 − X3 = 0 Equations (c) represent the components of the displacement vector at time t in the material description. To obtain the displacement in the spatial description, we substitute for X1 by use of (a) and obtain u1 =

x1 (a1 t + a2 t2 ) , 1 + a1 t + a2 t 2

u2 = 0,

u3 = 0

(d)

Equations (d) are the displacement components in the spatial description. For the velocity, we differentiate (a) with respect to t, keeping XR ﬁxed, to obtain v1 = X1 (a1 + 2a2 t),

v2 = 0,

v3 = 0

(e)

Equation (e) is in the material description and, for the spatial description, we eliminate X1 from (e) to obtain v1 =

x1 (a1 + 2a2 t) , 1 + a1 t + a2 t 2

v2 = 0,

We see that (f) is in the spatial description.

© 2005 by Chapman & Hall/CRC Press

v3 = 0

(f)

Motion and Deformation

3.3

83

Description of Deformation

We refer to the motion of a continuum when a body is undergoing change in geometry due to applied forces. The motion is generally described by the set of equations xi = xi (XR , t)

i = 1, 2, 3

(3.8)

These equations describe the change in position of a generic particle P with coordinates XR into p with coordinates xi . The functional relationship in (3.8) is generally nonlinear and its dependence on time t is discussed later in this chapter associated with material rate of change and rate of deformation. In this section, we study the deformation, that is, we set t to a constant time in (3.8). It is assumed that the mapping between XR and xi is one-to-one and onto; that is, for every particle in R0 there corresponds one point only in Rt and to every point in Rt there corresponds one particle only in R0 . Thus, the relation can be inverted to yield XR = XR (xi , t)

(3.9)

This assumption automatically satisﬁes the physical principle of conservation of mass and is a property of continuity. Motion described by (3.8) is the material description, where the variables are the material coordinates XR and time t; motion described by (3.9) is a spatial description, where the variables are xi and t. In this section, we study the deformation that has taken place at a speciﬁed time t. A special case of (3.8) is that xi is a linear function of XR such that xi = QiR (t)XR

(3.10)

If QiR is an orthogonal tensor, then QiR rotates vector XR into vector xi , which has been discussed in Section 1.6.2.

3.4

Deformation of a Neighborhood

Consider the deformation of a small material vector dX, which maps into vector dx in the deformed conﬁguration. Vector dX connects two neighboring points in neighborhood N0 and it may be considered as a line element between the two points. Due to deformation, the initial line element dX deforms into the current (deformed) line element dx and they are related by dx =

© 2005 by Chapman & Hall/CRC Press

∂x · dX = F · dX ∂X

(3.11)

84

Continuum Mechanics and Plasticity

where F = ∂x/∂X is called the deformation gradient, which plays an important role in modern continuum mechanics. In the component form, the deformation gradient F is written as F=

∂xi ei ⊗ eR = FiR ei ⊗ eR ∂XR

(3.12)

where eR and ei are base vectors of the material and special coordinate systems, respectively. Substituting (3.12) into (3.11), we have dxi ei =

∂xi ∂xi ∂xi ei ⊗ eR · dXS eS = dXS ei δRS = dXR ei ∂XR ∂XR ∂XR

(3.13)

Thus, the component form is obtained as dxi =

∂xi dXR = FiR dXR ∂XR

(3.14)

Note that the derivative ∂xi /∂XR is evaluated at point P and is common to all vectors dXR emanated from P within the neighborhood N0 . (In the mathematical expression f (x) = f0 + f (0)x + O(x2 ), the ﬁrst derivative f (0) is independent of x.) In the matrix form, (3.14) is written as x1,1 dx1 dx2 = x2,1 dx3 x3,1

x1,2 x2,2 x3,2

dX1 x1,3 x2,3 dX2 x3,3 dX3

(3.15)

and the Jacobian of the transformation is ∂xi J = ∂X

R

= det[F] = 0

(3.16)

If both xi and XR systems are right (or left) handed for all t, then det[F] > 0. This means that an inﬁnitesimal volume element (with ﬁnite value) cannot be deformed into a point. The volume change is discussed further later in this chapter. Some simple examples of ﬁnite deformation is considered in the concluding part of this section. We use ﬁnite versus inﬁnitesimal to distinguish large deformation from small deformation. In this chapter, most of our discussions are aimed at ﬁnite deformations. But, at the end of the chapter, we consider inﬁnitesimal deformation as a special case.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation 3.4.1

85

Homogeneous Deformations

Deformations of the form xi = ci + AiR XR

(3.17)

are homogeneous deformations. In (3.17), ci and AiR are constants or functions of time, but not functions of position XR . In this case, the deformation is the same for all points throughout the body being studied. We note that (3.17) is a linear form of the deformation equation (3.8). 3.4.1.1 Uniform extensions We consider a cube undergoing extensions in all three directions, so that x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

(3.18)

where λi specify the deformation and are constants or functions of time t. Note that (3.18) is a special case of (3.17). The deformation gradient of (3.18) may be found from (3.12) as

λ1 [F] = 0 0

0 λ2 0

0 0 λ3

(3.19)

If λ1 = λ2 = λ3 , the cube undergoes a uniform expansion or contraction in all directions and is referred to as a uniform dilatation. The volume of a material element in the cube was initially dV = dX1 dX2 dX3 and is now dv = dx1 dx2 dx3 = λ1 λ2 λ3 dX1 dX2 dX3 . Therefore, when there is no volume change, we write λ1 λ2 λ3 = 1. The volume change of an element is discussed further in a later section. In the case of an extension in the x1 direction of a long bar of uniform cross-section, λ2 = λ3 . When λ1 > 1, that is, stretching, it is usually observed that λ2 < 1. Note that λi > 0, because the length of a line element cannot become negative. 3.4.1.2 Simple shear In this deformation, parallel planes are displaced relative to each other with the distance between the planes unchanged. A square element is deformed into a parallelepiped. Thus, particle P with position vector X moves to p with position vector x as shown in Figure 3.2. The following set of equations describes a simple shear deformation: x1 = X1 + X2 tan γ ,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(3.20)

86

Continuum Mechanics and Plasticity x2

p

P

X x

x1

O FIGURE 3.2 Simple shear deformation.

where angle γ measures the amount of shear; the X2 = constant planes are the shear planes; and X1 is the shear direction. The deformation gradient of simple shear is found from (3.20) as

1 [F] = 0 0

3.4.2

tan γ 1 0

0 0 1

(3.21)

Nonhomogeneous Deformations

Equation (3.17) of homogeneous deformation leads to a deformation gradient F, which is not a function of position XR . Examples are (3.19) and (3.21). In the case of nonhomogeneous deformations, F is a function of position, that is, the deformation will be different from point to point. We consider torsion of a circular cylinder as an example of nonhomogeneous deformation. Referring to Figure 3.3, we choose the X3 axis to coincide with the axis of the cylinder. If the cylinder is twisted about the X3 axis, then plane cross-sections remain plane but are rotated rigidly through an angle τ X3 about the X3 axis. It is seen that this angle is proportional to the coordinate X3 , that is, the angle is zero at the base of the cylinder where X3 = 0 and increases its value as X3 increases. The quantity τ denotes the angle of twist per unit length and is a constant if the torque is applied at the two ends of the cylinder. In order to ﬁnd the equations of transformation that govern the deformation due to torsion, let us consider a typical cross-section shown in the insert of Figure 3.3. In the action of torsion, particle P(X1 , X2 , X3 ) with a radial distance R from the center of the circular section is rotated into p(x1 , x2 , x3 ), also with a radial distance R. At the initial position P, we have X1 = R cos α,

© 2005 by Chapman & Hall/CRC Press

X2 = R sin α,

1/2 with R = X12 + X22

(3.22)

Motion and Deformation

87

X3 R X3 p

X3

X2

P X1

Ο

X2

X1 FIGURE 3.3 Torsion of a circular cylinder.

After deformation at p, we write x1 = R cos(τ X3 + α),

x2 = R sin(τ X3 + α)

(3.23)

We then expand the cosine and sine functions in (3.23) and, by use of (3.22), obtain x1 = X1 cos τ X3 − X2 sin τ X3 ,

x2 = X1 sin τ X3 + X2 cos τ X3 ,

x2 = X3 (3.24)

Note that the equation in the 3-direction has been added due to the fact that the cross-section at a distance X3 from the base of the cylinder has merely undergone a rigid-body rotation. We conclude that (3.24) are the transformation equations that describe the deformation of a circular cylinder subjected to torsion. Differentiating (3.24), the deformation gradient F is found as

cos τ X3

[F] = sin τ X3 0

− sin τ X3 cos τ X3 0

−τ (X1 sin τ X3 + X2 cos τ X3 ) τ (X1 cos τ X3 − X2 sin τ X3 ) 1

(3.25)

It is seen that the deformation gradient depends on position for this nonhomogeneous problem. We have assumed in this discussion that the cylinder is undergoing a ﬁxed-end torsion. In this case, there is no length change in the cylinder and the radius R of the cylinder does not change. The free-end torsion is discussed in a later chapter related to plastic deformation.

© 2005 by Chapman & Hall/CRC Press

88

3.5

Continuum Mechanics and Plasticity

The Deformation Gradient

The deformation gradient plays an important role in modern continuum mechanics and is discussed in detail here. The deformation gradient F is a second-rank tensor; according to the polar decomposition theorem, a secondrank tensor can be expressed as a product of a positive symmetric tensor with an orthogonal tensor. There are two decompositions: the right and the left decompositions. They are expressed as F =R·U

right decomposition

(3.26)

F =V·R

left decomposition

(3.27)

where U and V are positive symmetric tensors, and R is an orthogonal tensor.

3.5.1

The Polar Decomposition Theorem

This theorem applies to any second-rank tensor, and there are the right and left decompositions as shown in (3.26) and (3.27). In this subsection, we consider a second-rank tensor Fij . This tensor acquires the physical meaning of deformation gradient in later sections. We now derive the right decomposition and consider tensor Fij transforms vector vi into vector vi ; the relation is vi = Fij vj

(3.28)

If the transformation (or mapping) is one-to-one, then the magnitude of vector vi is T |v |2 = vi vi = Fij Fik vj vk = Fki Fij vj vk > 0

(3.29)

T F is a posThis is a positive deﬁnite quadratic form. The coefﬁcient Ckj = Fki ij itive deﬁnite tensor. It is obvious that Ckj = Cjk . Since C is positive, a tensor √ U ≡ C is well deﬁned and it has the same eigenvectors as C. Thus,

U2 = FT · F ≡ C

(3.30)

Since C is symmetric, U is symmetric too. Now let R ≡ F · U−1 and it is seen that if we deﬁne R in this manner, then R is an orthogonal tensor. Using this expression for R, we have RT · R = (F · U−1 )T · (F · U−1 ) = (U−1 )T · FT · F · U−1 = U−1 · FT · F · U−1 = U−1 · C · U−1 = 1

© 2005 by Chapman & Hall/CRC Press

(3.31)

Motion and Deformation

89

Equation (3.30) is used in the last identity of (3.31). We see from (3.31) that R is an orthogonal tensor. In the above derivation, we also used the symmetric property of U and the relation (U−1 )T = U−1 . We have thus shown that F = R · U in which R is orthogonal and U is positive and symmetric. Following an analogous procedure, we derive the left decomposition. The resulting equations are F = V · R∗

and V2 = F · FT ≡ B

(3.32)

We now show that the orthogonal tensor R∗ of the left decomposition in the ﬁrst equation of (3.32) is indeed equal to the orthogonal tensor R of the right decomposition. From (3.32), we write F = V · R∗ = R∗ · (R∗T · V · R∗ )

(3.33)

and view the last expression in (3.33) as the right decomposition. Since the right decomposition is unique (see Example 3.2), we compare (3.33) with (3.26) to obtain R∗ = R

and U = RT · V · R

(3.34)

We see that U and V are related through equation (3.34). This relation can also be written as V = R · U · RT

(3.35)

Tensor B deﬁned in (3.32) can be shown to be related to tensor C deﬁned in (3.30). From the deﬁnition of B, we have B = F · FT = R · U · UT · R T = R · U2 · R T = R · C · R T

(3.36)

Hence, B = R · C · RT EXAMPLE 3.2

or

C = RT · B · R

(3.37)

Show that the right decomposition (3.26) is unique.

Proof Assume two decompositions exist: ¯ ·U ¯ F =R·U =R

(a)

¯T·R ¯T FT = UT · R T = U

(b)

Then, the transpose of (a) is

© 2005 by Chapman & Hall/CRC Press

90

Continuum Mechanics and Plasticity

Multiplying (a) and (b), we get ¯T·R ¯T ·R ¯ ·U ¯ FT · F = UT · R T · R · U = U ¯T·U ¯T = UT · U = U ¯2 = U2 = U

(c)

¯ and is positive. The uniqueness of R From (c), we conclude that U = U ¯ we conclude that R = R. ¯ follows from (a). Since U = U,

3.5.2

Polar Decompositions of the Deformation Gradient

If the tensor F in the previous subsection is assigned a physical meaning, then all the derived quantities have physical signiﬁcance. The polar decompositions of the deformation gradient F are F =R·U =V·R

FiR = RiS USR = Vij RjR

(3.38)

where F = deformation gradient = FiR ei ⊗ eR

(3.39a)

U = right stretch tensor = URS eR ⊗ eS

(3.39b)

V = left stretch tensor = Vij ei ⊗ ej

(3.39c)

R = rotation tensor (orthogonal tensor) = RiR ei ⊗ eR

(3.39d)

T

2

C = F · F = U = right Cauchy–Green deformation tensor, CRS = (∂xi /∂XR )(∂xi /∂XS )

(3.40)

B = F · FT = V2 = left Cauchy–Green deformation tensor, Bij = (∂xi /∂XR )(∂xj /∂XR )

(3.41)

where eR and ei are base vectors for the material and spatial system, respectively. We now discuss the physical meaning of the polar decompositions. The deformation gradient F deforms an element in two parts. In the right decomposition, the element is ﬁrst purely deformed to a quantity U. A rotation R then follows the deformation. This rotation represents the rotation of the principal axis of the stretch tensor U, which will be illustrated by Example 3.3. The above statement may be understood by applying F to a line element dX. Thus, dx = F · dX = R · (U · dX)

© 2005 by Chapman & Hall/CRC Press

(3.42)

Motion and Deformation

91

In the left decomposition, the element is ﬁrst rotated through R and then deformed by V. This statement may be veriﬁed by dx = F · dX = V · (R · dX)

(3.43)

The two modes of decomposition are fully equivalent. We obtain the same ﬁnal result. EXAMPLE 3.3

Consider a simple shear problem deﬁned by

x1 = X1 + kX2 ,

x2 = X2 ,

2 where k = √ 3

x3 = X3

(a)

(a) Find F, U, V, and R. (b) Use the right decomposition to draw ﬁgures showing the deformed state of the initially rectangular element at each stage of deformation. (c) Use the left decomposition to draw ﬁgures showing the deformed state of the initially rectangular element at each stage of deformation. (d) Study the deformation of a diagonal of the initially rectangular element. (e) Study the deformation of a circle in the initially rectangular element. Solution (a) Using (a), (3.39), and (3.40), we obtain 1 k 0 1 [F] = 0 1 0 , [F]T = k 0 0 1 0

0 0 1 0 , 0 1

1 1 k 0 T 2 2 [C] = [F] [F] = k (k + 1) 0 = √ 3 0 0 1 0

2 √ 3 7 3 0

(b)

0 0 1

(c)

To determine the principal values and directions of [C], we consider the characteristic equation

1 − λ 2 √ 3 0

© 2005 by Chapman & Hall/CRC Press

2 0 √ 3 n1 7 n2 = 0 −λ 0 3 n3 0 1−λ

(d)

92

Continuum Mechanics and Plasticity

By setting the determinant of the coefﬁcient matrix to 0, we obtain λ(i) = 3, 13 , 1. The corresponding eigenvectors are found to be

T nu(1)

=

√ 3 1 , ,0 , 2 2

3 1 , ,0 , = − 2 2

√

T nu(2)

nu(3) = [0, 0, 1] T

(e)

with the following transformation matrix between xi and xi (see (2.96)):

[Qu ] = nu(1)

(2)

nu

1 2

√ (3) nu = 3 2 0

√ − 3 2

0 0 1

1 2 0

(f)

These eigenvectors are shown in Figure 3.4 with φ = 60◦ . Referring to the principal axes xi , tensors C and U have components

3

[C ] = 0 0

0 0

0 1 3 0

√ 3 √ C = 0 and [U ] =

1

0

0 1 √ 3

0

0

1

0

(g)

It may also be veriﬁed that C is obtainable from the following transformation:

√ 3 1 2 2 √ T [C ] = [Qu ][C][Qu ] = − 3 1 2 2 0 0 3 0 0 1 = 0 0 3 0 0 1

0 1 2 √ 0 3 0 1

2 √ 3 7 3 0

1 0 2 √ 3 0 2 1 0

√ − 3 2 1 2 0

0 0 1

(h)

In addition, U can be determined by the following transformation: √ 3 2 [U] = [Qu ][U ][QuT ] = 1 2 0

© 2005 by Chapman & Hall/CRC Press

1 2 5 √

2 3 0

0 0 1

(i)

Motion and Deformation

93 2

n(1) = (cos , sin , 0)

n(2) = (–sin , cos , 0)

1

O FIGURE 3.4 Eigenvectors of C in simple shear deformation.

Since det[U] = 1, we ﬁnd

5 2√3 (cof[U])T [U −1 ] = = −1 det[U] 2 0

−1 2 √ 3 2 0

0 0 1

(j)

and [R] to be √ 3 2 [R] = [F][U −1 ] = −1 2 0

1 2 √ 3 2 0

0 0

(k)

1

The matrix in (k) describes a clockwise rotation of 30◦ of the continuum about the x3 axis. Note that √ √ 3 3 −1 1 0 0 1 0 0 2 2 2 2 √ √ T [R][R] = −1 (m) 1 = 0 1 0 3 3 0 0 0 0 1 2 2 2 2 0 0 1 0 0 1 which shows that RT = R−1 and R is therefore an orthogonal tensor. On the other hand, we may ﬁnd from the left decomposition 5 √ 2 3 [V] = [F][R−1 ] = 1 2 0

© 2005 by Chapman & Hall/CRC Press

1 2 √ 3 2 0

0

0 1

(n)

94

Continuum Mechanics and Plasticity

It may be easily shown that √ 3 [V ] = [U ] = 0 0

0 1 √ 3 0

0

0

(o)

1

and the principal directions of V are T n(1) v

√ 3 1 , , 0 , = 2 2

√ 3 1 , 0 , = − , 2 2

T n(2) v

n(3) = [0, 0, 1] v T

(p) with the transformation matrix given by (2) [Qv ] = n(1) nv v

(3)

(q)

nv

By use of (3.35), R rotates U into V. It also rotates vectors nu into nv . Putting all eigenvectors together in a matrix form, we may write √ √ √ 1 1 − 3 3 3 1 0 0 − 0 2 2 2 2 2 2 √ √ √ [Qv ] = [R][Qu ] = −1 3 = 1 3 3 1 0 0 0 2 2 2 2 2 2 0

0

1

0

0

1

0

0

1 (r)

All nu vectors that form Qu are rotated clockwise at a 30◦ angle into the nv vectors. This rotation is shown in Figure 3.5. (b) Consider a square element ABCD with unit side length, as shown in Figure 3.6. Using (3.42), the square ABCD is ﬁrst deformed by U into A B C D , which is subsequently rotated by R into A B C D . Thus, in the application n(2) v

2

nu(1)

nu(2)

n (1) v 30° 60° O

FIGURE 3.5 Rotation of nu into nv .

© 2005 by Chapman & Hall/CRC Press

1

Motion and Deformation

95 nu(1)

x2 C⬘ P⬘ B⬘ R B

C

P

B⬙

n(1) v P⬙

C⬙

D⬘ 30° A

60° D

x1

FIGURE 3.6 Right polar decomposition.

of U, line element AB is deformed into A’B’, AC into A C , etc. The deformed line elements are √ 1 1 3 0 2 2 2 0 √ 5 AB = 1 (s1) 5 3 1 = 0 √ 6 0 2 2 3 0 0 0 1 √ 3 1 0 1 1 2 2 √ 3 √ 5 AP = 1 (s2) = 3 0 1 √ 2 0 2 3 0 0 0 1 √ √ 1+ 3 1 3 0 2 2 2 1 √ 5 AC = 1 (s3) 1 = 3 + 5 3 0 √ 0 2 2 3 6 0 0 1 0 √ √ 3 1 3 0 2 2 1 2 5 A D = 1 (s4) 0 = 1 0 √ 0 2 2 2 3 0 0 1 0

© 2005 by Chapman & Hall/CRC Press

96

Continuum Mechanics and Plasticity

in which AP is a principal direction of U. Note that this method of ﬁnding the deformed shape of an element is valid only when F is not a function of position. If F is a function of position, then the line elements must be divided into small increments, and this method is applied to each increment. Alternatively, the set of transformation equations (3.8) may be used to ﬁnd the deformed shape of the element point by point. The rotation of A B C D into A B C D is obtained by applying R to the deformed line element A B , A P , etc. given by (s1 to s4). The resulting line elements are √ 3 2 A B = − 1 2 0 √ 3 2 A P = 1 − 2 0 √ 3 2 A C = 1 − 2 0 √ 3 2 A D = 1 − 2 0

1 2 √ 3 2 0 1 2 √ 3 2 0 1 2 √ 3 2 0 1 2 √ 3 2 0

1 √ 0 2 3 2 3 √ 5 3 = 1 0 6 0 0 1 0 √ 3 √1 = 1 3 0 0 0 1

(s5)

(s6)

√ 1+ 3 √ 0 3+2 3 2 √ 3 3 + 5 3 = 1 0 6 0 1 0 √ 3 0 1 2 0 = 1 0 0 2 0 1

(s7)

(s8)

The two stages of deformation and rotation are shown in Figure 3.6. (c) Using (4.43), the square ABCD is ﬁrst rotated into A B C D by R. √ 3 2 1 − 2 0

1 2 √ 3 2 0

0 0 1 0 0 1

© 2005 by Chapman & Hall/CRC Press

1 √ 3 1 0

1 1 1 2 √ = 1 0 3 2 0 0 0

1 1 √ 3 0

√ 1+ 3 2 √ −1 + 3 2 0

√ 3 2 1 − 2 0

(t1)

Motion and Deformation

97

Note that the ﬁrst matrix is R, the second matrix is formed by the column vectors AB, AP, AC, and AD, and the third matrix is a collection of column vectors A B , A P , A C , and A D . In the second step, the square A B C D is deformed into A B C D by V, given by the following equation √ 1 1+ 3 1 0 1 2 2 √2 √ √ 3 3 −1 + 3 1 0 √ 2 2 2 3 0 1 0 0 0 √ √ 3+2 3 2 3 √ 1 3 3 3 = 1 1 1 0 0 0 0 0

5 2√3 1 2 0

√ 3 2 1 − 2 0

(t2)

In equation (t2), the ﬁrst matrix is V, the second matrix consists of column vectors A B , A P , A C , and A D , and the third matrix is a collection of column vectors A B , A P , A C , and A D . The two stages of rotation and deformation are shown in Figure 3.7. Comparing (s5 to s8) with (t2), we see that the results obtained from the left decomposition is the same as those from the right decomposition.

x2

n(1) v C

B

P⬙

B⬙

C⬙

B⬘

C⬘

R 30° A

D

D⬘ FIGURE 3.7 Left polar decomposition.

© 2005 by Chapman & Hall/CRC Press

x1

98

Continuum Mechanics and Plasticity

(d) A straight line passing through the origin is given by X2 = X1 tan θ

(u)

where θ is the angle between the line and the X1 axis. Substituting (a) into (u), this line is deformed into 1 + k x2 (v) x1 = tan θ The diagonal of the initial square element has θ = 45◦ . This angle is deformed into α where tan α =

1 x2 = x1 1+k

(w)

(e) A circle in the initial element is given by X12 + X22 = a2

(x)

where a is the radius. Substituting (a) into (x), this circle is deformed into x12 − 2kx1 x2 + (1 + k 2 )x22 = a2

(y)

It is observed that a circle is deformed into an ellipse with the semimajor axis making an angle of β with√the positive x1 axis. It can be shown that tan 2β = 2/k. Thus, when k = 2/ 3, β = 30◦ .

3.6

The Right Cauchy–Green Deformation Tensor

We now discuss some popular strain measures. Any strain measure is as good as the other as long as its deﬁnition is clear and correctly used. It is a matter of convenience to choose one measure over another for the description of the problem at hand. We discuss in this section a popular strain measure called the right Cauchy–Green tensor. Other popular measures are discussed in sections 3.9 and 3.10.

3.6.1

The Physical Meaning

Consider a line element dXR with length dS deforming into dxi with length ds. We have dxi =

© 2005 by Chapman & Hall/CRC Press

∂xi dXR ∂XR

(3.44)

Motion and Deformation

99

Dividing both sides of (3.44) by (ds dS), we obtain λni =

∂xi NR ∂XR

dXR dS

and ni =

(3.45)

where NR =

dxi ds

(3.46)

specify the directions (unit vectors) of the line element before and after deformation, respectively. The extension ratio (or stretch ratio) λ is deﬁned by λ=

ds dS

(3.47)

The notation λ is a popular notation for stretch ratio and should not be confused with the eigenvalues used in Chapter 2. Because of many notations, symbols, and quantities, the same notation may be used to mean different quantities. You should pay special attention to the deﬁnition of each notation used. Using (3.45), we form λ2 = (λni )(λni ) =

∂xi ∂xi NR NS = CRS NR NS ∂XR ∂XS

(3.48)

or λ2 = CRS NR NS

(3.49)

Note that CRS is a symmetric tensor and is positive deﬁnite. Given a deformation (3.8), F and C may be found. If we specify the initial direction NR of a line element, then the direction and magnitude of the deformed line element may be found using (3.45) and (3.49), respectively. In order to visualize the meaning of the diagonal terms C11 , C22 , C33 and the (1) off diagonal terms C12 , C23 , etc., of CRS , let us consider two line elements dXR (2) (1) (2) and dXR , which deform into dxi and dxi , respectively. The angle between the two line elements is in the initial conﬁguration and φ in the current conﬁguration as shown in Figure 3.8. The initial and deformed line elements are related by (1)

dxi

(2)

dxi

© 2005 by Chapman & Hall/CRC Press

∂xi (1) dXR ∂XR ∂xi (2) = dXR ∂XR =

(3.50) (3.51)

100

Continuum Mechanics and Plasticity

Then, we form the inner product of the two line elements (1)

(2)

dxi dxi

=

∂xi ∂xi (1) (2) (1) (2) dXR dXS = CRS dXR dXS ∂XR ∂XS

(3.52)

On the other hand, the inner product may be expressed in terms of the lengths of the line elements and the angle φ as (1)

(2)

dxi dxi

= ds1 ds2 cos φ12

(3.53)

where ds1 and ds2 are the lengths of the two line elements after deformation and φ12 is the inclusion angle. Let dS1 and dS2 be the lengths of the two line elements before deformation, then (1)

dXR (1) = NR dS1

(2)

dXR (2) = NR dS2

(3.54)

Using (3.54) and equating (3.52) to (3.53), we obtain ds1 ds2 (1) (2) cos φ12 = CRS NR NS dS1 dS2

(3.55)

From (3.55), we obtain information for C11 , C22 , C33 . Let us consider a line (1) (1) (1) element oriented initially along X1 , then N1 = 1, N2 = 0, N3 = 0. In this case, (3.55) reduces to

ds1 dS1

2

(2)

= C11 = λ1

(3.56a)

We note that C11 is related to the extension ratio λ1 along X1 . Similarly, if we consider line elements oriented initially along X2 and X3 , respectively, we obtain C22 =

ds2 dS2

2

and C33 =

ds3 dS3

2 (3.56b,c)

We now consider the angle changes between the two line elements as shown in Figure 3.8. In a special case, the two line elements are initially 90◦ (2) (1) to each other. Let dXi be along the X1 direction and dXi be along the (1) (2) X2 direction, then the unit normals are NR ∼ [1, 0, 0] and NS ∼ [0, 1, 0]. Equation (3.55) now reduces to ds1 ds2 cos φ12 = C12 dS1 dS2

© 2005 by Chapman & Hall/CRC Press

(3.57)

101

i

dx (1

)

Motion and Deformation

(1)

dX R

(2)

dx i

Φ

dX

(2 R )

FIGURE 3.8 Deformation of two line elements.

Making use of (3.56), (3.57) becomes cos φ12 = √

C12 √

C11 C22

(3.58)

Note that (3.58) relates C12 to φ12 , which is the angle after deformation. The angle φ12 may no longer be 90◦ and the two line elements are in general not oriented along the coordinate axes after deformation. Using a similar procedure, we relate C23 to φ23 and C31 to φ31 . These equations are summarized and we write cos φRS = √

CRS √ CRR CSS

(R, S not summed)

(3.59)

It may be concluded that the diagonal terms C11 , C22 , C33 are related to the extension ratios λ1 , λ2 , λ3 , respectively; they represent the stretching along the coordinate directions; the off-diagonal terms C12 , C23 , C31 are related to the current angles φRS , respectively; they are different from the initial angles RS and, therefore, represent shearing deformation. Finally, we remark that, if the triad formed by the three initial line elements are along the principal directions of CRS , then C12 = C23 = C31 = 0. From (3.59), we ﬁnd φ12 = φ23 = φ31 = 90◦ , that is, the triad remains mutually perpendicular to each other after deformation. Furthermore, in the undeformed state, CRS does not vanish, that is, C11 = 1, C22 = 1, C33 = 1, and C12 = cos φ12 = 0, etc., or we may write CRS = δRS in the undeformed conﬁguration.

3.6.2

Transformation Properties of CRS

In this subsection, we consider the transformation properties of CRS with respect to the rotation and translation of either the material coordinate system ¯ R be an alternative material system, or the spatial coordinate system. Let X

© 2005 by Chapman & Hall/CRC Press

102

Continuum Mechanics and Plasticity

which is related to XR by ¯ R = MSR XS + aR X

(3.60)

where MRS is a rotation matrix, that is, MTR MTS = δRS = MRT MST

with |MRS | = 1

(3.61)

Both M and a are independent of XR . Also, let x¯ i be an alternative spatial system such that x¯ i = Qji (t)xj + bi (t)

(3.62)

where Qij Qik = δjk = Qji Qki

with |Qij | = 1

(3.63)

¯ R and x¯ i differs from the original system by a rigid-body Note that each of X rotation plus a translation. 3.6.2.1 Rotation and translation of material system ¯ R , the expressions of CRS are, respectively, Referring to XR and X CRS =

∂xi ∂xi ∂XR ∂XS

and

∂xi ∂xi C¯ RS = ¯ R ∂X ¯R ∂X

(3.64)

By the chain rule of differentiation, we have CRS =

¯ T ∂xi ∂ X ¯V ∂xi ∂xi ∂ X ∂xi = MRT M = MRT MSV C¯ TV ¯ ¯ ¯ ¯ V SV ∂ XT ∂XR ∂ XV ∂XS ∂ XT ∂X

(3.65)

or C¯ RS = MTR MVS CTV

(3.66)

Therefore, CRS transforms as a second-order tensor with rotation of the material system but it remains invariant with translation of the material system. This result is expected because both subscripts of CRS refer to the material system. We note that C¯ RS in this subsection should not be confused with the C¯ RS matrix referring to the principal coordinate system and used in most other sections.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

103

3.6.2.2 Rotation and translation of the spatial system Referring to xi and x¯ i , the expressions of CRS are, respectively, CRS =

∂xi ∂xi ∂XR ∂XS

and CRS =

∂ x¯ i ∂ x¯ i ∂XR ∂XR

(3.67)

The second equation in (3.67), by use of (3.62), is further written as CRS =

∂xj ∂ x¯ i ∂xj ∂ x¯ i ∂xk ∂xk = Qji Qki ∂xj ∂XR ∂xk ∂XS ∂XR ∂XS

= δjk

∂xj ∂xk ∂xk ∂xk = = CRS ∂XR ∂XS ∂XR ∂XS

(3.68)

We conclude that CRS remains invariant with rotation and translation of the spatial system. This is also expected, because both subscripts of CRS refer to the material system and it does not matter which spatial coordinate system we use.

3.6.3

Eigenvalues and Eigenvectors of CRS

CRS is a symmetric matrix and it has three real eigenvalues and three real eigenvectors. The properties of eigenvalues and eigenvectors are discussed ¯ R to denote the principal coordinate system of CRS . in Section 2.7. We use X The principal values (eigenvalues) C¯ RS are related to CRS by

C¯ RS = QPR QQS CPQ

ds1 dS1 = 0 0

2

0 ds2 dS2 0

2

2 λ1 =0 0 0 ds3 2 0

0

0

λ22

0

0

λ23

dS3 (3.69)

We see that, when CRS are expressed in the principal frame, it becomes a (R) diagonal matrix. The eigenvectors, or the principal directions, are nC with R = 1, 2, and 3. Figure 3.9 shows the eigenvectors in the neighborhood N0 of an undeformed body. Whatever the deformation of N0 , there exists one set of three line elements, which are mutually orthogonal. The three line elements may extend during deformation and the triad may rotate, but the angles between them will always be right angles.

© 2005 by Chapman & Hall/CRC Press

104

Continuum Mechanics and Plasticity

nC(3) N0

nC(2) nC(1)

R0 3 2 1

FIGURE 3.9 Eigenvectors in the neighborhood N0 .

3.6.4

Principal Invariants of CRS

Similar to the stress invariants discussed in Section 2.12, we deﬁne the invariants for CRS as (3.70) I1 = CRR = C11 + C22 + C33 I2 = tr(cof. C) = I3 tr(C−1 )

(3.71)

I3 = det C

(3.72)

We now discuss the geometric signiﬁcance of I1 , I2 , and I3 . In principal axes, the invariants I1 , I2 , and I3 may be associated with the geometric properties of a material element. The matrix of C is a diagonal matrix as shown in (3.69). In this system, the expressions for the invariants are I1 = λ21 + λ22 + λ23

(3.73)

I2 = λ22 λ23 + λ21 λ23 + λ21 λ22 1 1 1 1 1 1 = λ21 λ22 λ23 + 2 + 2 = I3 + 2 + 2 = I3 tr(C−1 ) λ21 λ2 λ3 λ21 λ2 λ3 I3 = λ21 λ22 λ23

(3.74) (3.75)

In the case that the initial lengths are dS1 = 1, dS2 = 1, and dS3 = 1, (3.69) reduces to

ds21 C= 0 0

© 2005 by Chapman & Hall/CRC Press

0 ds22 0

0 0 ds22

(3.76)

Motion and Deformation

105

ds3

3

P 2

O

ds 1

d s2

1 FIGURE 3.10 Deformed cuboid for geometric interpretations of strain invariants.

and I1 = |OP|2 = ds21 + ds22 + ds23

(3.77)

I2 = sum of squares of areas of three mutually perpendicular faces of deformed cuboid 2 ds 0 ds21 0 ds21 2 = + + 0 ds2 0 ds2 0 3

3

0 = ds22 ds23 + ds21 ds23 + ds21 ds22 ds2 2

(3.78) I3 = square of volumes of deformed unit cuboid = (ds1 ds2 ds3 )

2

(3.79)

The above geometric interpretations are clear when we refer to Figure 3.10.

3.7

Deformation of Volume and Area of a Material Element

We investigate ﬁrst the deformation of a volumetric element within the neighborhood N0 and then investigate how an area element deforms during deformation. The initial volume of an inﬁnitesimal parallelepiped within N0 is dV0 , which is the scalar triple product of the three vectors

© 2005 by Chapman & Hall/CRC Press

106

Continuum Mechanics and Plasticity

forming the sides of the parallelepiped. The deformed volume is denoted by dV. We have (1) (2) (3) dV0 = dX(1) · dX(2) × dX(3) = ePQR dXP dXQ dXR

(3.80)

∂xi (1) ∂xj (2) ∂xk (3) dXP dXQ dXR ∂XP ∂XQ ∂XR ∂xi ∂xi ∂xj ∂xk (1) (2) (3) dX (1) dX (2) dX (3) = eijk dXP dXQ dXR = ePQR Q R ∂XP ∂XQ ∂XR ∂XP P (3.81) (1)

(2)

(3)

dV = eijk dxi dxj dxk = eijk

From (3.80) and (3.81), we obtain ∂xi dV = ∂X

P

dV0

or

∂xi dV = det F = dV0 ∂XP

(3.82)

Let dm be the mass of the volumes dV and dV0 and ρ and ρ0 be the densities of dV and dV0 , respectively. Equation (3.82) may be rewritten as ∂xi ρ0 = det F = J = ρ ∂XP

(3.83)

∂xi ∂xi = |FT · F| = |FT | |F| = |F|2 I3 = |CRS | = ∂XR ∂XS

(3.84)

Now that

we ﬁnd from (3.83) and (3.84) that I3 =

dV dV0

2

=

ρ0 ρ

2 (3.85)

We consider next the deformation of an area element. Referring to Figure 3.11, (2) (1) line elements dXR and dXR form the initial area dA, which has a unit (1) (2) normal of NR . The two line elements deform into dxi and dxi , and area dA deforms into da with unit normal ni . The two areas can be expressed as vectors given by dAR = NR dA

© 2005 by Chapman & Hall/CRC Press

and

dai = ni da

(3.86)

Motion and Deformation dA R N =

M⬙

R dA

d

) (2 XR

d

M

107

=n

id

a

ai

dA

m⬙ ) (2 dx i

dX (1) R

da

m dx (1) i

M⬘

m⬘ (After Deformation)

(Before Deformation) FIGURE 3.11 Deformation of area element.

In addition, the undeformed area is (1)

(2)

with (dA)2 = dAR dAR

(3.87)

(1)

(2)

with (da)2 = dai dai

(3.88)

dAR = eRST dXS dXT and the deformed area is dai = eijk dxj dxk

We now proceed to ﬁnd the relation between the two areas. By way of the chain rule of differentiation, (3.87) can be written as dAR = eRST

∂XS ∂XT (1) (2) dx dxn ∂xm ∂xn m

(3.89)

Multiplying (3.89) by ∂XR /∂xk , we obtain ∂XS ∂XT ∂XR (1) (2) ∂XM ∂XR (1) dAR = eRST dxm dxn = dxn(2) ekmn dxm ∂xk ∂xm ∂xn ∂xk ∂xr ∂XM dak = (3.90) ∂x r

Equation (3.88) and the identity discussed in Example 2.7 have been used in the above derivation. Thus, we may conclude that ∂XM ∂XR dak dAR = ∂xk ∂xr

(3.91)

or using (3.83), dai = J

∂XR dAR ∂xi

or

da = J(F−1 )T · dA

Equation (3.92) relating dAR to dai is called Nanson’s formula.

© 2005 by Chapman & Hall/CRC Press

(3.92)

108

3.8

Continuum Mechanics and Plasticity

The Left Cauchy–Green Deformation Tensor

The left Cauchy–Green tensor B is deﬁned in (3.41). It is seen that both subscripts of Bij refer to the spatial coordinate system. B is invariant with rotation of the material system and transforms as a second-rank tensor with rotation of the spatial system. We now show that the invariants of B, denoted by IB , II B , and III B , coincide with those of C, denoted by IC = I1 , II C = I2 , and III C = I3 . From (3.70), we have ∂xi ∂xi = Bii = IB ∂XR ∂XR

IC = CRR =

(3.93)

and from (2.79), the second invariant is II B =

1 2

IB2 − tr B2

(3.94)

where B2 = Bip Bpj and the trace of this expression is ∂xi ∂xp ∂xp ∂xi tr B = Bip Bpi = = ∂XR ∂XR ∂XS ∂XS 2

∂xi ∂xi ∂XR ∂XS

= CRS CRS = tr C2

∂xp ∂xp ∂XR ∂XS

(3.95)

Substituting (3.93) and (3.95) into (3.94), we obtain II B = II C

(3.96)

For the third invariant, we have from (3.72) and (3.84) III C = |C| = |FT · F| = |FT ||F| = |F|2

(3.97)

III B = |F · FT | = |F||FT | = |F|2

(3.98)

On the other hand,

Comparing (3.97) and (3.98), we ﬁnd III B = III C

3.9 3.9.1

(3.99)

The Lagrangian and Eulerian Strain Tensors Deﬁnitions

The two classical strain measures discussed in this section are widely used in mechanics literature. Usually, they are derived from a different approach

© 2005 by Chapman & Hall/CRC Press

109

P

dX

u

dx

Motion and Deformation

p Nt

X

N0

x

3 2 1 FIGURE 3.12 The displacement vector.

than the one given here. Having discussed the right and left Cauchy–Green deformation tensors, we may deﬁne the Lagrangian and Eulerian strains as 2E = C − 1

(3.100)

2e = 1 − B−1

(3.101)

where E is the Lagrangian strain tensor (also known as Green’s tensor) and e is the Eulerian strain tensor. We point out, from (3.100), that C is positive for E > − 12 . In this discussion, we observe that deformation of a continuum may be described by different strain measures. In fact, there are several alternative measures of deformation that are being used in the literature. The displacement vector u introduced in (3.3) is now considered. Refer to Figure 3.12 and let the material and spatial coordinate systems coincide for simplicity. If a material point P moves to p during deformation, the vector from P to p is the displacement vector u. We may write x =X+u

or

xi = δiR XR + ui

(3.102)

Using (3.102), (3.100) becomes ∂xm ∂xm − δRS ∂XR ∂XS ∂ (δmM XM + um ) ∂ (δmN XN + um ) = − δRS ∂XR ∂XS ∂um ∂um δmS + − δRS = δmR + ∂XR ∂XS

2ERS = CRS − δRS =

= δmR δmS + δmR

© 2005 by Chapman & Hall/CRC Press

∂um ∂um ∂um ∂um + δmS + − δRS ∂XS ∂XR ∂XR ∂XS

(3.103)

110

Continuum Mechanics and Plasticity

Note that we choose to have the origin of the material and spatial coordinate systems coincide. In general, they may not coincide, but since the vector connecting the two origins is a constant, it drops out in the differentiation. Thus, (3.103) may be simpliﬁed to yield ERS

1 = 2

∂uS ∂uR ∂uk ∂uk + + ∂XS ∂XR ∂XR ∂XS

(3.104)

Equation (3.104) is known as the strain–displacement relation. Similarly, from (3.101), we obtain 1 eij = 2

∂uj ∂uR ∂uR ∂ui + − ∂xj ∂xi ∂xi ∂xj

(3.105)

where uR and ui are respectively components of the displacement vector u in the material and spatial coordinate systems. Since both coordinate systems are Cartesian and coincide in this consideration, uR is the same as ui . Also, XR is the same as Xi . Some remarks are in order. 1. Both ERS and eij are symmetric tensors. 2. A line element dXR with length dS in the neighborhood of N0 deforms into dxi with length ds in the neighborhood of Nt . It is possible to show that ds2 − dS2 = 2ERS dXR dXS = 2eij dxi dxj

(3.106)

3. For small deformation, that is, ∂ui /∂XR 1, and ∂uR /∂xj 1, but ui may not be small, we can approximately write 1 Eij ∼ = 2

∂uj ∂ui + ∂Xj ∂Xi

1 ∼ = eij ∼ = 2

∂uj ∂ui + ∂xj ∂xi

= εij

(3.107)

It is not necessary to distinguish the material coordinates XR from the spatial coordinates xi (see Example 3.4). The tensor εij is called the inﬁnitesimal strain tensor or the engineering strain. Both E and e reduce to ε when an approximation is made such that the second and the higher powers of the displacement gradients are neglected. 4. On the other hand, the inﬁnitesimal strain tensor may be mathematically deﬁned by 1 εij = 2

© 2005 by Chapman & Hall/CRC Press

∂uj ∂ui + ∂xj ∂xi

(3.108)

Motion and Deformation

111

Physically, ε cannot be an exact measure of deformation, because it does not remain constant in a rigid-body rotation. In a counterclockwise rigid-body rotation through an angle α about the positive X3 axis, the transformation of the position vector of a material point is given by (see Example 1.6) x1 = X1 cos α − X2 sin α,

x2 = X1 sin α + X2 cos α,

x3 = X3 (3.109)

and the displacement components are u1 = −X1 (1 − cos α) − X2 sin α, u2 = X1 sin α − X2 (1 − cos α),

u3 = 0

(3.110)

Using (3.108), the inﬁnitesimal strain ε is determined to be

−(1 − cos α) 0 0 −(1 − cos α) εij = 0 0

0 0 0

(3.111)

It is seen that ε11 and ε22 are not 0. However, if α is small, then these quantities are small and may be neglected. Although the inﬁnitesimal strain tensor is not an exact measure of deformation, it is convenient for use in the applications involving small strains. An advantage of this strain tensor is its linear relation with respect to the displacement gradient. This allows for the application of the techniques of linear analysis in solving boundary-value problems in the linear theory of elasticity, and also helps keep the equations of the theory of plasticity simple. Nevertheless, in using (3.108), we must keep in mind that the rigid-body rotation has to be small. Show that, in the case of small displacement gradient, we may write ∂ui /∂xj ∼ = ∂ui /∂Xj and it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi .

EXAMPLE 3.4

Solution From (3.102), we have xi = Xi + ui

(a)

∂ui ∂Xi = δij − ∂xj ∂xj

(b)

By differentiating (a), we obtain

© 2005 by Chapman & Hall/CRC Press

112

Continuum Mechanics and Plasticity

In the symbolic notation, (b) can be written as ∂u = 1 − F−1 = 1 − {1 + (F − 1)}−1 ∂x = 1 − {1 − (F − 1) + (F − 1)2 − (F − 1)3 + · · · } = (F − 1) − (F − 1)2 + (F − 1)3 − · · ·

(c)

in which the binomial expansion was used. In the index notation, the factor (F − 1) is ∂xi ∂ui − δij = ∂Xj ∂Xj

(d)

∂ui ∂ui ∂ui ∂uR ∂ui ∂uR ∂uS = − + − ··· ∂xj ∂Xj ∂XR ∂Xj ∂XR ∂XS ∂Xj

(e)

By substitution, (c) becomes

Hence, by neglecting the higher-order terms in the displacement gradient, we may write ∂ui ∼ ∂ui = ∂xj ∂Xj

(f)

and it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi . 3.9.2

Geometric Interpretation of the Strain Components

We consider here as in Section 3.6.1 a line element dXR with length dS deforming into dxi with length ds. We relate the stretching of this line element to the components of E rather than to the components of C. From the usual deﬁnition of strain, we deﬁne the relative elongation of the line element as ε=

ds − dS ds = −1=λ−1 dS dS

(3.112)

This deﬁnition of relative elongation is valid for large deformation as well. From (3.106), we have ds2 = dS2 + 2ERS dXR dXS

(3.113)

Dividing (3.113) by dS2 , we obtain λ2 =

dXR dXS ds2 = 1 + 2ERS = 1 + 2ERS NR NS dS dS dS2

© 2005 by Chapman & Hall/CRC Press

(3.114)

Motion and Deformation

113

or λ = [1 + 2ERS NR NS ]1/2

(3.115)

where NR denotes the initial direction of the line element. We have discarded the “−” solution in (3.115), since λ = ds/dS ≥ 0 always. Therefore, the relative elongation is from (3.112) given by ε = λ − 1 = [1 + 2ERS NR NS ]1/2 − 1

(3.116)

If we know ERS and specify a direction NR , then from (3.116) we obtain the elongation of this line element. Equation (3.115) may be compared with (3.49), in which the components of C are used. These expressions show that the extension ratio can be obtained by the use of two different strain measures. The two equations are related by λ2 = 1 + 2ERS NR NS = NR NR + 2ERS NR NS = (δRS + 2ERS )NR NS = CRS NR NS

(3.117)

We now consider the meaning of the diagonal and off-diagonal components of the ERS matrix. To discuss the diagonal component E11 , let us consider a line element in the X1 direction before deformation. We then have N1 = 1, N2 = 0, and N3 = 0; and, from (3.114), we obtain λ211 = 1 + 2E11

and ε11 = λ11 − 1 =

1 + 2E11 − 1

(3.118)

Equation (3.118) shows that E11 is related to the stretching of the line element, which is initially in the X1 direction. Similarly, if we consider line elements initially along X2 and X3 directions, respectively, we get ε22 =

1 + 2E22 − 1

and ε33 =

1 + 2E33 − 1

(3.119)

Starting with the Eulerian strain components eij , we can also obtain expressions for the relative elongations for ﬁbers, which after deformation are in the directions of the x1 , x2 , and x3 axes. However, the interpretation of e11 , e22 , and e33 as the relative elongations of ﬁbers can only be justiﬁed for small strain. If we choose a line element, which is in the x1 direction after deformation, then (3.106) leads to (ds − dS)(ds + dS) = 2eij dxi dxj = 2e11 n1 n1 ds2 = 2e11 ds2

(3.120)

By use of the deﬁnition of relative elongation, (3.120) may be written as ds − dS ds 2ds = e11 ≈ e11 dS dS ds + dS © 2005 by Chapman & Hall/CRC Press

(3.121)

114

Continuum Mechanics and Plasticity

The last expression of (3.121) is true only for small deformation that ds ≈ dS. In this case, e11 may be interpreted as the relative elongation for ﬁbers in the x1 direction, and we note that for small deformation x1 ≈ X1 . However, in large deformation, no simple correlation between e11 and relative elongation can be found from (3.121). To investigate the off-diagonal terms of ERS , let us consider two line (1) (2) (1) (2) elements dXR and dXR , which deform into dxi and dxi , respectively. The angle between the two line elements is in the initial conﬁguration and (1) φ in the current conﬁguration as shown in Figure 3.8. The dot product of dXR (2) and dXR is (1)

(2)

dS1 dS2 cos = dXR dXR (1)

and the dot product of dxi

(2)

and dxi

(3.122)

is (1)

(2)

ds1 ds2 cos φ = dxi dxi

(3.123)

Subtracting (3.122) from (3.123), we obtain (1)

(2)

(1)

(2)

ds1 ds2 cos φ − dS1 dS2 cos = dxi dxi − dXR dXR ∂xi ∂xi (1) (2) = − δRS dXR dXS ∂XR ∂XS ∂ui ∂ui (1) (2) = + δiR + δiS − δRS dXR dXS ∂XR ∂XS (1)

(2)

= 2ERS dXR dXS

(3.124)

The relations in (3.103) are used in the derivation of (3.124). Dividing the above expression by dS1 dS2 , we obtain (1)

(2)

dXR dXS ds1 ds2 (1) (2) cos φ − cos = 2ERS = 2ERS NR NS dS1 dS2 dS1 dS2

(3.125)

This relation may be further simpliﬁed by use of (3.112), which, for the two line elements, are ds1 = λ1 dS1

and

ds2 = λ2 dS2

(3.126)

Using (3.126), (3.125) may be solved to yield (1)

cos φ =

© 2005 by Chapman & Hall/CRC Press

(2)

2ERS NR NS + cos λ1 λ 2

(3.127)

Motion and Deformation

115

where is the angle between the two line elements before deformation (1) (2) and φ is the angle after deformation. Given , ERS , NR , and NS , the deformed angle φ may be determined. Note that the stretch ratios λ1 and λ2 are determined from (3.115). To investigate the meaning of E12 , E23 , E31 , let us consider some special cases. If = 90◦ , that is, the two line elements are perpendicular to each other before deformation, then cos = 0. In addition, let cos φ = cos(90◦ − θ ) = sin θ, where θ is the angle change due to deformation, then (3.127) reduces to (1)

sin θ =

(2)

2ERS NR NS λ 1 λ2

(3.128)

Since θ is generally not 0 from (3.128), we may conclude that two initially perpendicular line elements (not along the coordinate axes) do not remain perpendicular after deformation. If the two line elements are respectively (1) (1) (1) lying along the X1 and X2 axes initially, then N1 = 1, N2 = N3 = 0 and (2) (2) (2) N2 = 1, N1 = N3 = 0, and from (3.128) E12 is related to θ12 . Similarly, we ﬁnd the expressions for other off-diagonal terms of ERS (R = S). The relations are summarized as sin θ12 =

2E12 , λ1 λ 2

sin θ23 =

2E23 , λ 2 λ3

sin θ13 =

2E13 λ 1 λ3

(3.129)

We observe from (3.129) that the off-diagonal terms of ERS are related to the shearing deformations and that an initially orthogonal triad with elements along the XR directions will no longer be orthogonal after deformation. We consider a special case, where X1 , X2 , and X3 are principal directions. Then, E12 = E23 = E31 = 0 and E11 = E1 , E22 = E2 , E33 = E3 . If the two line elements are respectively lying along X1 and X2 initially, then from (3.129) we obtain θ12 = 0, which means that there is no angle change, that is, φ = = 90◦ . Similarly, we show that θ23 = θ31 = 0. This ﬁnding has the implication that a rectangular triad having elements in the three principal directions before deformation remains rectangular (does not have angle changes) after deformation. The volume element formed by the triad is rotated and may be stretched. However, if, before deformation, the triad is in directions other than the principal directions, then there are angle changes after deformation even if ERS refers to the principal directions. The angle changes for this case are calculated from (3.128).

3.9.3

The Volumetric Strain

Using (3.82) and (3.100), we have

dV dV0

© 2005 by Chapman & Hall/CRC Press

2

= |FT · F| = |C| = |δRS + 2ERS |

(3.130)

116

Continuum Mechanics and Plasticity

Since the above expression is the third invariant of C, a simpliﬁed expression is obtained by using the principal coordinate system. Thus,

dV dV0

2

= (1 + 2E1 ) + (1 + 2E2 )(1 + 2E3 ) = 1 + 2(E1 + E2 + E3 ) + 4(E1 E2 + E1 E3 + E2 E3 ) + 8E1 E2 E3 (3.131)

or

dV dV0

2

= 1 + 2IE + 4II E + 8III E

(3.132)

where IE , II E , and III E are the principal invariants of E. But, from (3.116), we note that 1 + ε1 =

1 + 2E1

(3.133)

in which ε1 is the relative elongation along principal direction 1. Using (3.133), (3.131) becomes dV = (1 + ε1 )(1 + ε2 )(1 + ε3 ) = λ1 λ2 λ3 dV0

(3.134)

We note that the volumetric strain for small deformation is dV − dV0 dV = − 1 = (1 + ε1 )(1 + ε2 )(1 + ε3 ) − 1 ≈ ε1 + ε2 + ε3 (3.135) dV0 dV0 by neglecting the high-power terms in ε1 , ε2 , or ε3 . In the ﬁnite deformation, the volumetric strain can be deﬁned by (dV − dV0 )/dV, which leads to the logarithmic volumetric strain of ln(dV). EXAMPLE 3.5

Consider the deformation governed by x 1 = α1 X 1 ,

x2 = α2 X2 ,

x3 = α3 X3

(a)

where αi are constants. In a one-dimensional stretching along the 1 direction, determine the values of E11 , e11 , the relative elongation ε, and the true strain εlog , if α1 takes the values of 1.01, 1.02, 1.05, 1.10, and 1.20. Compare these values with the engineering strain ε eng .

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

117

Solution Using (a), we ﬁnd

α12 T [C] = [F] [F] = 0 0

0 α22 0

0 0 α32

and [B]−1

1 α2 1 = 0 0

0 1 α22 0

0

0 1

(b)

α32

Substituting (b) into (3.100) and (3.101), we obtain (C11 − 1) = 12 (α12 − 1) 1 1 1 −1 1− 2 = (1 − B11 ) = 2 2 α1

E11 = e11

1 2

(c) (d)

Since N1 = 1, N2 = N3 = 0, the relative elongation ε may be found from (3.116) and (c) as ε = α1 − 1

(e)

Note that this result is the same as that obtained from the deﬁnition of engineering strain, where ε eng =

x−X = α1 − 1 X

(f)

The true strain is deﬁned by dε log = dx/x. If the initial strain is 0 and the initial length of the specimen is X, this expression may be integrated to ﬁnd ε log = ln

x X

= ln α1

(g)

Expressions (c) to (g) are plotted in Figure 3.13 against α1 . The curve for the engineering strain εeng is a straight line. The curve for E11 lies above the straight line and the curves for εlog and e11 lie below the straight line. We note that, at a strain of εeng = 0.05, the corresponding logarithmic strain is εlog = 0.0488, which is 2.4% smaller than ε eng ; at εeng = 0.1, ε log = 0.0953, which is 4.9% smaller than εeng ; and at εeng = 0.2, ε log = 0.1823, which is 9.7% smaller than εeng .

© 2005 by Chapman & Hall/CRC Press

118

Continuum Mechanics and Plasticity E11 e11

0.2

eng log

Strain

0.15 0.1 0.05 0 1.0

1.15

1.1 1

1.05

1.2

FIGURE 3.13 Comparison of strain measures in one-dimensional stretching.

3.10

Other Strain Measures

Several other strain measures have been used in the literature. We mention in this section two families of strains, which are deﬁned based on the stretch tensors U and V discussed in Section 3.5. Both U and V are positive, symmetric tensors, they share the same eigenvalues λi and their eigenvectors are related by the transformation given by equation (r) of Example 3.3. In the proposed strain measures, the eigenvalues are a function of λi such that εi = f (λi )

(3.136)

A useful form for function f is given by λκi − 1 , κ = ln λi ,

f (λi ) =

κ = 0

(3.137)

κ=0 (i)

(i)

The two families of strains are written using either nu or nv as their eigenvectors. Thus, E = f(U) =

f (λi )nu(i) ⊗ nu(i)

i

or

e = f(V) =

f (λi )nv(i) ⊗ nv(i)

i

(3.138) where E may be called the generalized Lagrangian strain and e the generalized Eulerian strain. Some commonly used strain measures may be

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

119

obtained from (3.138). They are Engineering strain (κ = 1): ε eng = λ − 1 Logarithmic strain (κ = 0):

ε log = ln λ

Lagrangian strain (κ = 2):

E = 12 (λ2 − 1) 1 1 e= 1− 2 2 λ

Eulerian strain (κ = −2):

(3.139)

The last two strain measures are written in the spectral form as E=

1 i

2

(λ

2

− 1)nu(i)

⊗ nu(i)

and e =

1 1 − 2 nv(i) ⊗ nv(i) 2 λ

1 i

(3.140)

A disadvantage of strain measures deﬁned by (3.138) is the necessity of calculating the principal components ﬁrst and then performing axes transformation to the actual axes. A popular method to avoid axes transformation is to use strain measures with κ = 2 or −2 so that the strain tensors may be directly calculated from either the stretch tensors U and V or the right and left Cauchy–Green tensors C and B.

3.11

Material Rate of Change

We discussed the concept of deformation and its measures in the earlier sections. As mentioned earlier, the deformation describes the geometrical change of a material element between the current and the reference conﬁgurations corresponding to two different ﬁxed times. The study now extends to the motion of the body, which is a family of deformations continuously varying in time. The material rate of change (or material derivative) is an important concept used in the description of the motion and we discuss it in this section. The material rate of change of a physical quantity φ is the rate of change of φ with respect to a particle. This rate is also known as the substantial derivative in ﬂuid mechanics. There are material and spatial descriptions for the material rate of change and we discuss them in this section.

3.11.1

Material Description of the Material Derivative

In the material description, X is held constant, and the material derivative is the same as the partial derivative with respect to time t. Therefore, we write D ∂φ(X, t) φ(X, t) = Dt ∂t

© 2005 by Chapman & Hall/CRC Press

(3.141)

120

Continuum Mechanics and Plasticity

or in the index notation D ∂φ(XR , t) φ(XR , t) = Dt ∂t 3.11.2

(3.142)

Spatial Description of the Material Derivative

In the spatial description, φ is a function of x and t. The material derivative of φ is the total derivative of φ, differentiating with respect to both variables. Thus, D ∂φ(x, t) ∂φ ∂x φ(x, t) = + · Dt ∂t ∂x t ∂t X

(3.143)

Note that the last differentiation is carried out by keeping X constant. This is so because we are considering the material derivative. The particle velocity has been discussed in (3.6), and using the expression, (3.143) becomes D ∂φ(x, t) −−−−→ φ(x, t) = + Grad φ · v(x, t) Dt ∂t

(3.144)

In the last expression of (3.144), notation v represents v(x, t). The same notation v may be used to represent v(X, t) in the material description. These are actually two different functions denoting the same velocity. But for the sake of simplicity in notations, we use the same notation v. The independent variables of the function should be speciﬁed in case confusion arises. In a similar manner, we discuss the material differentiation of a vector. Acceleration, which is the material derivative of the velocity vector, is a good example and is given by f=

Dv ∂v = + (Grad v) · v Dt ∂t

(3.145)

The last expression of (3.145) may be derived by writing Grad v ≡

∂vi ei ⊗ e j ∂xj

=∇ ⊗v

(3.146)

Thus, (Grad v) · v = =

© 2005 by Chapman & Hall/CRC Press

∂vi ∂vi ei ⊗ ej · vk ek = vk ei (ej · ek ) ∂xj ∂xj

∂vi ∂vi vk ei δjk = vk ei ∂xj ∂xk

(3.147)

Motion and Deformation

121

Using (3.147), the index form of (3.145) is fi =

∂vi ∂vi Dvi = + vk Dt ∂t ∂xk

(3.148)

Generally, the material derivative in the spatial description is represented by the following operator D ∂ ∂ = + vk Dt ∂t ∂xk

(3.149)

If this operator is applied to a function φ(x, t), then the ﬁrst term indicates the local rate of change, which is the contribution of the time dependence of φ. This term may also be called the transient term. The second term is the convective term, which is the contribution by the motion of the particle. To illustrate this point, let us consider ﬂuid ﬂowing in a tube and we assume that the ﬂow is steady and is one-dimensional along the x direction (see Figure 3.14). In a steady ﬂow, the velocity at any location x does not change with time. The observer sitting at a location x does not see any change of v, so that ∂v/∂t = 0. However, the velocity may differ from one location to the other. The acceleration of the particle is then given by Acceleration =

change of velocity (∂v/∂x)x (∂v/∂x)vt ∂v = = =v time increment t t ∂x (3.150)

This acceleration is known as the convective acceleration and is due to the motion of the ﬂuid. In a nonsteady ﬂow, the velocity changes with time at a ﬁxed station x. It changes from v to v + (∂v/∂t)t in time interval t and the acceleration at this station x is given by Acceleration =

change of velocity (∂v/∂t)t ∂v = = time increment t ∂t ∆x = v∆t

x t =t velocity v = v FIGURE 3.14 Fluid ﬂowing in a tube.

© 2005 by Chapman & Hall/CRC Press

x + ∆x t = t + ∆t ∆v velocity = v + ∆x ∆x

(3.151)

122

Continuum Mechanics and Plasticity

This is the transient term of acceleration and there is no convective acceleration because we consider the acceleration at a ﬁxed station. In the general case, that is, the station is not ﬁxed at x and the ﬂow is nonsteady, the total acceleration is therefore f=

∂v ∂v +v ∂t ∂x

(3.152)

In summary, the material rate of change, which is the rate of change of a physical quantity with respect to a speciﬁed particle, can be speciﬁed either by using a material description or a spatial description. In the material description, XR is speciﬁed and the particle is colored red. The material rate for a physical quantity is seen by an observer sitting on top of the particle and moving with the particle. Thus, the material rate changes with respect to t only. In the spatial description, the spatial coordinate changes (convects) with the particle, and the material rate of change has two parts, the convective and the transient. Thus, the acceleration of a speciﬁed (red) particle is what an observer who stands still in the laboratory sees.

3.12

Dual Vectors and Dual Tensors

The concept of dual vector and dual tensor is useful in the subsequent sections of this chapter. Given a tensor of the second-rank Tij , let us form the following vector ti = − 12 eijk Tjk

(3.153)

Vector ti is called the dual vector (or axial vector) of tensor Tij . We can show that the dual vector depends only on the antisymmetric part of tensor Tij . Thus, ti = − 12 eijk Tjk = − 12 eijk TjkS + TjkA = − 12 eijk TjkA

(3.154)

in which the superscripts S and A denote the symmetric and the antisymmetric parts, respectively. We note that the dual vector of a symmetric tensor vanishes and it has the components given below T − T32 1 23 T31 − T13 t=− 2 T −T 12

(3.155)

21

which forms a column vector. If we multiply both sides of (3.153) by eijk , we obtain eijk ti = − 12 eijk eirs Trs = − 12 (δjr δks − δjs δkr )Trs = − 12 (Tjk − Tkj )

© 2005 by Chapman & Hall/CRC Press

(3.156)

Motion and Deformation

123

Therefore, if Tij is symmetric, then from (3.156), ti = 0; and if Tij is antisymmetric, eijk ti = −Tjk , that is, Tjk = −eijk ti

(3.157)

Tjk is called the dual tensor of a given vector ti and the dual tensor is antisymmetric with components given by

0 T = t3 −t2

−t3 0 t1

t2 −t1 0

(3.158)

Use the dual vector–dual tensor concept to describe the angular velocity of rigid-body rotation of a continuum.

EXAMPLE 3.6

Solution Let us consider a rigid body that instantaneously rotates about an axis passing through point P in the body, and P has position vector r0 (see Figure 3.15). Note that for an inﬁnitesimal rotation, we consider the increments of angular and linear displacements dθ and dx, respectively, instead of angular and linear velocities ω = dθ/dt and v = dx/dt and similar results may be obtained. The vector ω shown speciﬁes the magnitude of angular velocity ω, the direction of the axis of rotation, and the sense of rotation. The velocity of point A speciﬁed by position vector r is then v = ω × (r − r0 )

(a)

ω

v

r – r0 P r0

O FIGURE 3.15 Angular velocity in rigid-body rotation.

© 2005 by Chapman & Hall/CRC Press

r

A

124

Continuum Mechanics and Plasticity

In the index notation, (a) is written as (0)

vi = eijk ωj (xk − xk )

(b)

From vector ω we deﬁne its dual tensor as jk = −eijk ωi

(c)

Substituting (c) into (b), we obtain (0)

vi = ik (xk − xk )

or

v = · (r − r0 )

(d)

We see that the angular velocity can be represented either by vector ω or tensor .

3.13

Velocity of a Particle Relative to a Neighboring Particle

We consider two particles P and P in a continuum in motion. The coordinate of P is XR initially, and xi at time t. For the sake of simplicity, the origins and axes of the material and spatial coordinate systems coincide. The coordinate of P is XR + XR initially, and xi + xi at time t. The line element between the two particles is dXR initially and dxi at time t. The initial and deformed line element are related by dxi =

∂xi dXR ∂XR

(3.159)

The relative velocity of P with respect to P is dvi ≡ vi (P , t) − vi (P, t) = vi (XR + dXR , t) − vi (XR , t) = v˜ i (xj + dxj , t) − v˜ i (xj , t)

(3.160)

in which the particle velocity is either expressed in the material description by the use of function vi (XR , t) or in the spatial description by the use of function v˜ i (xi , t). From the material description, (3.160) may be further written as dvi =

D [xi (XR + dXR , t) − xi (XR , t)] Dt

(3.161)

Observing that dxi denotes the line element connecting two adjacent material particles, (3.161) reduces to dvi =

© 2005 by Chapman & Hall/CRC Press

D (dxi ) Dt

(3.162)

Motion and Deformation

125

It is seen from (3.162) that the order of differentiation between d and D/Dt is interchangeable. Using the spatial description, from (3.160), we write dvi = v˜ i (xj + dxj , t) − v˜ i (xj , t)

(3.163)

The ﬁrst term on the right-hand side may be expanded in Taylor’s series and, by retaining only the ﬁrst-order term, (3.163) becomes dvi = v˜ i (xj , t) +

∂ v˜ i ∂ v˜ i dxk − v˜ i (xj , t) = dxk = vi,j dxj ∂xk ∂xk

(3.164)

Combining (3.162) and (3.164), we obtain dvi =

D(dxi ) = vi,j dxj Dt

(3.165)

where vi,j = Lij is known as the velocity gradient tensor. This tensor is generally not symmetric and so it can be split into symmetric and antisymmetric parts. Therefore, we write Lij = vi,j = 12 (vi,j + vj,i ) + 12 (vi,j − vj,i ) = Dij + Wij

(3.166)

where Dij = 12 (vi,j + vj,i )

or

D = 12 (L + LT )

(3.167)

Wij = 12 (vi,j − vj,i )

or

W = 12 (L − LT )

(3.168)

and

in which Dij is the rate of deformation tensor and Wij is the spin tensor. Therefore, (3.165) may be rewritten as dvi = Dij dxj + Wij dxj

3.14

(3.169)

Physical Signiﬁcance of the Rate of Deformation Tensor

In order to see the physical signiﬁcance of the rate of deformation tensor Dij , (1) (2) let us consider two material line elements, dxi and dxi , at the current conﬁguration in the spatial system. Let φ be the angle formed by the two line (1) (2) elements, with unit vectors ni and ni and lengths ds1 and ds2 , respectively.

© 2005 by Chapman & Hall/CRC Press

126

Continuum Mechanics and Plasticity (1)

(2)

We then differentiate the inner product dxi dxi to yield

of the two line elements

D (1) (2) (1) (2) (1) (2) (1) (2) dxi dxi = vi,j dxj dxi + dxi vi,j dxj = dxi dxj [vi,j + vj,i ] Dt (3.170) or D (1) (2) (1) (2) dxi dxi = 2Dij dxi dxj Dt (1)

(2)

On the other hand, since dxi dxi equation by differentiation,

(3.171)

= ds1 ds2 cos φ, we obtain the following

D D Dφ D (1) (2) dxi dxi = (ds1 )ds2 cos φ + ds1 (ds2 ) cos φ − ds1 ds2 sin φ Dt Dt Dt Dt (3.172) Equating (3.171) and (3.172), and dividing the resulting equation by ds1 ds2 , we obtain 1 D 1 D Dφ (1) (2) (ds1 ) cos φ + (ds2 ) cos φ − sin φ = 2Dij ni nj ds1 Dt ds2 Dt Dt

(3.173)

Note that ni = dxi /ds in the above equation. Special cases may be deduced from (3.173). If the two line elements coincide, then φ = 0 and ds1 = ds2 = ds. In this case, (3.173) reduces to 1 D (ds) = Dij ni nj ds Dt

(3.174)

The expression on the left-hand side of (3.174) is precisely the deﬁnition of true strain-rate, which is the rate of length change per unit length at the current conﬁguration. Knowing Dij and specifying a direction ni , the strainrate along this direction may be found from (3.174). Using the concept of stretch ratio λ = ds/dS, where dS does not change with time, (3.174) may be expressed as λ˙ = Dij ni nj λ

(3.175)

In particular, let ni = (1, 0, 0), then (1/ds1 )((D/Dt)ds1 ) = λ˙ 1 /λ1 = D11 , where D11 is time rate of change (extension or contraction) per unit length of an element, which at time t is oriented along the x1 axis. A similar interpretation applies to D22 and D33 .

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

127

To see the physical meaning of the off-diagonal terms of the Dij matrix, let φ = 90◦ in (3.173). Then, the two line elements are perpendicular to each other at time t. In this case, (3.173) reduces to − (1)

In particular let ni

Dφ (1) (2) = 2Dij ni nj Dt (2)

be along the x1 axis and ni −

(3.176) be along x2 , then

Dφ = 2D12 Dt

(3.177)

It is seen that D12 is the shear rate. The quantity −Dφ/Dt is the rate of change (1) (2) of the right angle between the two elements dxi and dxi . The negative sign means that the angle φ is decreasing. If we let θ = 90◦ − φ, then Dθ/Dt = −Dφ/Dt, that is, θ is increasing. A similar interpretation applies to D13 and D23 . Show that the necessary and sufﬁcient condition for rigidbody motion of a continuum is Dij = 0.

EXAMPLE 3.7

Proof The length ds of a deformed line element is ds2 = dxi dxi

(a)

Material differentiation of (a) yields D D D (ds2 ) = (dxi dxi ) = 2 (dxi )dxi = 2vi,j dxj dxi Dt Dt Dt

(b)

where we used (3.165). We observe that the last expression of (b) is symmetric in i and j and it may be further written as D (ds2 ) = (vi,j + vj,i )dxi dxj = 2Dij dxi dxj Dt

(c)

In (c), dxi is a vector connecting two neighboring points and it is arbitrary and nonzero. The quantity D(ds2 )/Dt is 0, if and only if Dij = 0. But D(ds2 )/Dt = 0 implies that the length of an arbitrary line element in a body does not change, which precisely is the deﬁnition for a rigid body.

© 2005 by Chapman & Hall/CRC Press

128

3.15

Continuum Mechanics and Plasticity

Physical Signiﬁcance of the Spin Tensor

Consider a pure rigid-body rotation, which is a special case of motion of a continuum. Let the motion be described by xi = QiR (t)XR

(3.178)

where QiR is a function of time t and is orthogonal such that QiR (t)QjR (t) = δij ,

QiR (t)QiS (t) = δRS ,

and |QiR | = 1

(3.179)

Differentiating (3.178) with respect to time, we obtain ˙ iR XR vi = Q

˙ iR = d QiR where Q dt

(3.180)

In the above expression, the velocity is expressed in the material system XR that does not change with time. On the other hand, the velocity may be expressed in the spatial description. To show this, we invert (3.178) to yield XR = QjR xj

(3.181)

By substitution, we obtain from (3.180) and (3.181) ˙ iR QjR xj vi = Q

(3.182)

We see that the velocity is in the spatial description in (3.182). If we differentiate the ﬁrst equation of (3.179), we ﬁnd ˙ iR QjR = −QiR Q ˙ jR ij = Q

(3.183)

From (3.183), we see that the quantity ij is antisymmetric. Substituting this result back into (3.182), we ﬁnd that rigid-body rotation of a continuum is governed by the following velocity ﬁeld vi = ij (t)xj

(3.184)

At any instant of time t, the increment of (3.184) can be compared with (3.165) and (3.169). This can be seen in the case of rigid-body rotation Lij = Wij = ij and Dij = 0, where the spin tensor can be identiﬁed with the angular velocity of the rigid-body motion. The angular velocity tensor ij is further related to the velocity gradient through (3.168). Since ij is antisymmetric, it has only

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

129

three nonzero independent components in the off-diagonal terms. In terms of the dual vector ωk as in (3.158), the matrix of ij is

ω2 −ω1 0

−ω3 0 ω1

0 ij = ω3 −ω2

(3.185)

Also, using (3.157), we form eijm ij = −eijm eijk ωk = −2δmk ωk

(3.186)

ωk = − 12 eijk ij

(3.187)

or

Substituting (3.157) into (3.184), the particle velocity is now given by vi = −eijk ωk xj = ekji ωk xj

or

v =ω×x

(3.188)

where ω is the angular velocity vector of the rigid-body rotation. We note that in a general motion of a continuum, W is not equal to and is determined by (3.168), expressed in terms of velocity gradients. The dual vector of W is given by wk = − 12 eijk 21 (vi,j − vj,i ) = − 12 eijk vi,j = 12 ejik vi,j

(3.189)

or w=

1 2

Curl v

(3.190)

This is the vorticity vector, which is frequently used in ﬂuid mechanics.

3.16

Expressions for D and W in Terms of F

Although (3.167) and (3.168) may be used to describe a continuum undergoing general motions, we derive here the expressions of D and W in terms of the deformation gradient F. We do this because F has been used extensively in the description of deformation. The velocity gradient L may be written as L=

∂v ∂v ∂X = · = F˙ · F−1 = −F · (F−1 )· ∂x ∂X ∂x

© 2005 by Chapman & Hall/CRC Press

(3.191)

130

Continuum Mechanics and Plasticity

where the last equality has been obtained from the differentiation of F · F−1 = 1. If we use the right polar decomposition of F given by (3.26), then (3.191) becomes L = −(R · U) · ((R · U)−1 )· = −R · U · (U−1 · R−1 )· = −R · U · [(U−1 )· · R−1 + U−1 · (R−1 )· ] = −R · U · (U−1 )· · RT − R · R˙ T ˙ · U−1 · RT + R ˙ · RT =R·U

(3.192)

In the derivation of (3.192), we recognized the relation R−1 = RT and used the results obtained from the differentiation of relations U · U−1 = 1 and R · RT = 1. We now take the transpose of (3.192) to yield ˙ · U−1 )T + (R ˙ · R T )T LT = R · (R · U

(3.193)

Therefore, from (3.192) and (3.193), we obtain ˙ · U−1 + U−1 · U) ˙ · RT D = 12 (L + LT ) = 12 R · (U

(3.194)

and ˙ · U−1 − U−1 · U) ˙ · RT + R ˙ · RT W = 12 (L − LT ) = 12 R · (U

(3.195)

Similarly, by use of the left polar decomposition (3.27), we may show that ˙ · V−1 + V−1 · V ˙ +V·R ˙ · RT · V−1 − V−1 · R ˙ · RT · V) D = 12 (V

(3.196)

and ˙ · V−1 − V−1 · V ˙ +V·R ˙ · RT · V−1 + V−1 · R ˙ · RT · V) W = 12 (V

(3.197)

Show that the spin tensor W describes the angular velocity of the principal axes of the rate of deformation tensor D.

EXAMPLE 3.8

Proof Let ni be a normalized eigenvector of Dij and ni = dxi /ds. We take the material derivative of ni and write D n˙ i = Dt

dxi ds

= vi,j nj −

=

dxi 1 D 1 1 D 1 D (dxi ) − 2 (ds)dxi = vi,j dxj − (ds) ds Dt ds ds Dt ds ds Dt

λ˙ ni = vi,j nj − Djk nj nk ni = (Dij + Wij )nj − Djk nj nk ni λ

© 2005 by Chapman & Hall/CRC Press

(a)

Motion and Deformation

131 D (ds)/dS and Dt (for p = 1, 2, 3) the eigenvectors of Dij , we write

Note that, in the derivation of (a), we used λ = ds/dS, λ˙ = (p)

(3.175). Denoting by ni

(p)

(Dij − D(p) δij )nj

=0

(b)

where D(p) is the corresponding principal value of Dij . Using (b), we replace (p)

(p)

(p) (p)

Dij nj by D(p) ni , and using relation ni nj may be written as (p)

n˙ i

(p)

= D(p) ni

(p)

+ Wij nj (p)

= −eijm wm nj

= δij given by (2.86), equation (a) (p) (p) (p)

− D(p) nk nk ni (p)

= eijk wj nk

(p)

= Wij nj

(c)

In the symbolic notation, (c) is written as n˙ (p) = w × n(p)

(d)

This expression shows that w is the angular velocity of n(p) , which is a principal direction of the rate of deformation tensor D.

3.17

Material Derivative of Strain Measures

We introduced several strain measures in earlier sections of this chapter. In this section, we explore the relationships between the material derivatives, denoted by a dot, of C and E and the rate of deformation D. Let us differentiate (3.40) ﬁrst to obtain ∂xi ∂vi ∂vi ∂xi ∂xi ∂vi ∂xk ∂vi ∂xk ∂xi C˙ RS = + = + ∂XR ∂XS ∂XR ∂XS ∂XR ∂xk ∂XS ∂xk ∂XR ∂XS ∂vi ∂xi ∂xk ∂vk ∂xi ∂xk = + = 2Dik (3.198) ∂xk ∂xi ∂XR ∂XS ∂XR ∂XS We then differentiate (3.100) and ﬁnd 2E˙ RS = C˙ RS

(3.199)

Summarizing (3.198) and (3.199), we have ∂xi ∂xk 1 E˙ RS = C˙ RS = Dik 2 ∂XR ∂XS

(3.200)

Equation (3.200) relates the material derivatives E˙ RS and C˙ RS to the rate of deformation Dij .

© 2005 by Chapman & Hall/CRC Press

132

Continuum Mechanics and Plasticity

EXAMPLE 3.9

Show that the material derivative of the Jacobian is given by DJ ∂vk =J Dt ∂xk

(a)

Proof DJ D|∂xi /∂XR | ∂J ∂J D(∂xk /∂XS ) ∂vk ∂xm = = = Dt Dt ∂(∂xk /∂XS ) Dt ∂(∂xk /∂XS ) ∂xm ∂XS Using (2.76), the expression ∂J/∂ and according to (2.84), we write

∂xk ∂XS

in (b) is the cofactor of matrix

∂J ∂XS =J ∂xk ∂(∂xk /∂XS )

(b) ∂xk ∂XS ,

(c)

Substituting (c) into (b), we obtain (a).

3.18

Material Derivative of Area and Volume Elements

We ﬁrst ﬁnd the material derivative of an area element. The deformed and initial areas are related by Nanson’s formula (3.92), and the differentiation of (3.92) leads to D DJ ∂XR D D ∂XR ∂XR (dai ) = dAR dAR = +J J Dt Dt ∂xi Dt ∂xi Dt ∂xi

(3.201)

Deriving an expression to represent the last term of (3.201), we differentiate the expression ∂xi ∂XR = δij ∂XR ∂xj

(3.202)

to obtain D Dt

∂xi ∂XR

∂XR ∂xi D + ∂xj ∂XR Dt

∂XR ∂xj

=0

(3.203)

This equation may be further simpliﬁed to yield ∂vi ∂xi D + ∂xj ∂XR Dt

© 2005 by Chapman & Hall/CRC Press

∂XR ∂xj

=0

(3.204)

Motion and Deformation

133

which reduces to D Dt

∂XR ∂xj

=−

∂vi ∂XR ∂xj ∂xi

(3.205)

Substituting (3.205) and the expression of Example 3.9 into (3.201) to obtain D (dai ) = Dt

=J

DJ ∂XR D +J Dt ∂xi Dt

∂XR ∂xi

dAR

∂vk ∂XR ∂vk ∂XR ∂vk ∂vk dAR − J dAR = dai − dak ∂xk ∂xi ∂xi ∂xk ∂xk ∂xi

(3.206)

we may conclude that the material rate of an area element is D ∂vk ∂vk (dai ) = dai − dak Dt ∂xk ∂xi

(3.207)

Finally, let us consider the material derivative of the volume element. Since dV = J dV0 , we can differentiate the equation to obtain D(dV) D DJ ∂vk ∂vk = (JdV0 ) = dV0 = J dV0 = dV = Dkk dV Dt Dt Dt ∂xk ∂xk

(3.208)

The material derivative of the logarithmic volumetric strain is then D 1 D(dV) [ln(dV)] = = vk,k = Div v = Dkk Dt dV Dt

(3.209)

All of the last three forms in (3.209) have been used in the continuum mechanics literature. When there is no volume change, we have from (3.208) or (3.209), vk,k = Dkk = Div v = 0. This is a necessary and sufﬁcient condition for the material element to undergo no volume change. We note that a material element undergoing no volume change is merely a geometrical condition. It has no implication as to whether the material is compressible or not. But, when a material element does not suffer any volume change in all loading conditions, the material is then incompressible.

References 1. Truesdell, C. and Toupin, R. S. Flugge (ed.) The Classical Field Theories, in Handbuch der Physik, Vol. III/1, Springer-Verlag, Berlin, 1960. 2. Spencer, A.J.M., Continuum Mechanics, Longman, London and New York, 1980. 3. Chadwick, P., Continuum Mechanics, George Allen & Unwin, London, 1976. 4. Eringen, A.C., Mechanics of Continua, Wiley, New York, 1967.

© 2005 by Chapman & Hall/CRC Press

134

Continuum Mechanics and Plasticity

Problems (1) In the deformation deﬁned by x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

ﬁnd the expressions for the following tensors: F, C, U, R, where λi are constants. If λ1 = 1.2, λ2 = 0.8, and λ3 = 1, sketch the deformed shape of a unit cube. (2) In the deformation of problem 1 with λ1 = 1.2, λ2 = 0.8, and λ3 = 1, determine the deformed length of a diagonal connecting point O (0, 0, 0) to point C (1, 1, 1). Determine also the ﬁnal orientation of this diagonal. (3) Consider the following deformation and refer to Figure 3.16 x1 = λ1 X1 + X2 tan γ ,

x2 = λ2 X2 ,

x3 = λ3 X3

where λi and γ are constants. Sketch the deformed shape of square OABC in the X1 − X2 plane. The sides are initially of unit length.

X2

C

O

B

A

X1

X3 FIGURE 3.16

(4) For the simple shearing deformation given by x1 = X1 +kX2 , x2 = X2 , x3 = X3 , where k is a constant, ﬁnd the components of C in terms of k and determine the eigenvalues and eigenvectors of C. Discuss the eigenvalues and eigenvectors of C as k varies from negative to positive and from small to large values. (5) For the simple shearing deformation given by x1 = X1 +kX2 , x2 = X2 , x3 = X3 , where k is a constant, represent by a sketch the deformed area to which the

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

135 X3

C (0, 0, 1)

B (0,1,0)

O

(1, 0, 0)

X2

A

X1 FIGURE 3.17

original area OABC transforms (see Figure 3.17). Obtain an expression to describe the direction of the line element OA after deformation. (6) Consider the following deformation x1 =

√ 2X1 + 43 X2 ,

x2 = X1 − 43 X2 + 41 X3 ,

x3 =

√ 2X3

Find (a) the direction after the deformation of a line element, which is initially oriented with a direction ratio 1:1:1; (b) the stretch ratio of this line element. (7) By use of the imaging-based method, the locations of the four corners of a twodimensional, initially square, material element have been determined after deformation. The initial and deformed elements are shown in Figure 3.18. Using the property that F transforms undeformed line elements into deformed line elements, determine the components of F and C.

D (0, 1)

C⬘ (1.3, 1.1) D⬘ (0.5, 0.9)

C (1, 1)

(0.8, 0.2) B⬘ A (0, 0) FIGURE 3.18

© 2005 by Chapman & Hall/CRC Press

B (1, 0)

136

Continuum Mechanics and Plasticity X3

A

O

B

X2

D

C

X1 FIGURE 3.19 Figure for Problem 11.

(8) Show that

cos θ FiR = sin θ 0

− sin θ cos θ 0

0 0 1

describes a rigid-body rotation. (9) A square element is subjected to a uniaxial extension in the 1 direction, and is then rotated about the positive 3 direction through an angle of 90◦ . Determine the deformation gradient F. (10) In the case of plane strain, experimental measurements give stretch ratios λ of 0.8 and 1.2 in the X1 and X2 directions, respectively, and 0.6 in the direction making a 45◦ angle with the X1 axis. Determine the components of C and E. (11) Consider the unit cube shown in Figure 3.19, which undergoes the deformation x1 = α X1 − 12 X2 ,

x2 = βX2 ,

x3 = γ X3

where α, β, and γ are constants. Determine (a) the deformed length of diagonal OA (b) the angle between OB and OD after deformation (c) the condition that constants α, β, and γ must satisfy if the material is incompressible. (12) For the deformation of Problem (11), determine the expressions for components of tensors F, C, U, V, R, B, E, and e. Use α = 1.2, β = γ = 0.9.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

137

(13) In the case of simple shear deformation of a square block governed by x1 = X1 + kX2 ,

x2 = X2 ,

x3 = X3

where k is constant, determine the extension ratios for the sides and the diagonals. Find the volume of the block before and after deformation. (14) The most general two-dimensional homogeneous deformation is deﬁned by the following linear transformation x1 = aX1 + bX2 ,

x2 = cX1 + dX2 ,

x3 = X3

Find components of C, B, and E in terms of constants a, b, c, and d. (15) Consider the following deformation and refer to Figure 3.16 x1 = X1 + 12 X22 ,

x2 = X2 ,

x3 = X3

(a) Sketch the deformed shape of square OABC in the X1 − X2 plane. The sides are initially of unit length. (b) Consider at point O two line elements: dX(1) = dX(1) e1 and dX(2) = dX(2) e2 . Find the deformed line elements dx(1) and dx(2) , and calculate the dot product dx(1) · dx(2) . Determine the change in the original right angle between dX(1) and dX(2) due to deformation. (c) Do the same thing as in (b) for two line elements dX(1) = dX(1) e1 and dX(2) = dX(2) e2 located at point C. (16) In the initial conﬁguration, a circular cylinder with radius R has its axis aligned with the X3 direction. If the cylinder undergoes the deformation x1 = α{X1 cos(τ X3 ) + X2 sin(τ X3 )} x2 = α{−X1 sin(τ X3 ) + X2 cos(τ X3 )} x3 = βX3 determine the conditions that need to be satisﬁed by constants α, β, and τ so that the volume is preserved during deformation. Determine the length of a line element in the deformed conﬁguration, which initially has unit length and lies on the surface of the cylinder along the X3 direction. Determine also the initial length of a line element on the surface of the cylinder that, in the deformed conﬁguration, has unit length and lies in the X3 direction. (17) For an isotropic material, the coefﬁcient of thermal expansion is αij = αδij , where α is a constant. A line element of length L elongates an amount dL if the temperature is raised by dT, so that dL = αdTL. For a block of L1 × L2 × L3 subjected to this change in temperature, write down the set of three transformation equations that describes this deformation. Find the components of F and determine the current length of a diagonal of the block, which had an initial length of L.

© 2005 by Chapman & Hall/CRC Press

138

Continuum Mechanics and Plasticity

(18) If the eigenvalues for U are λ(i)• = 3, 13 , 1 and the corresponding eigenvectors are

√

√ 3 3 1 1 (1)T (2)T (3)T nu = , ,0 , nu = − , ,0 , nu = (0, 0, 1) 2 2 2 2 use E = f(U) =

i

(i)

(i)

f (λi )nu ⊗ nu with f (λi ) =

λκi −1 to determine the κ

components of E with respect to the XR system when κ = 2 and −2. (19) If the eigenvalues for V are λ(i) = 3, 13 , 1 and the corresponding eigenvectors are

√

√ 1 3 1 3 (1)T (2)T (3)T nv = , , 0 , nv = − , , 0 , nv = [0, 0, 1] 2 2 2 2 (i) (i) use e = f(V) = i f (λi )nv ⊗nv with f (λi ) = (λκi −1)/κ to determine the components of e with respect to the xi system when κ = 2 and −2. Assume that XR and xi coincide for simplicity. (20) Consider a rectangular triad before deformation. Discuss what would happen to this triad after deformation. Would it remain rectangular? Under what condition? (21) Let the displacement ﬁeld be given by u1 = 41 (X3 − X2 ),

u2 = 41 (X1 − X3 ),

u3 = 41 (X2 − X1 )

Determine the volume ratio dV/dV0 . (22) Show that the velocity ﬁeld v1 = 2x3 − 3x2 ,

v2 = 3x1 − x3 ,

v3 = x2 − 2x1

corresponds to a rigid-body rotation. Determine this rotation by a vector so that we know the axis of rotation. (23) Consider the motion x1 = X1 + 12 X22 t,

x2 = X2 ,

x3 = X3

At t = 0, the corners of a unit square are at O (0, 0, 0), A (1, 0, 0), B (1, 1, 0), and C (0, 1, 0). Sketch the deformed shape of square OABC in the X1 − X2 plane when t = 1 and when t = 2. (24) For the motion of Problem (23), determine the velocity and acceleration of a particle in both material and spatial descriptions. (25) For the motion of Problem (23), determine the expressions for L, D, and W. (26) For the velocity ﬁeld v1 = −αx2 , v2 = αx1 , v3 = β, where α and β are constants, ﬁnd the components of tensors L, D, and W.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

139

(27) Let a velocity ﬁeld be described by vi = αxj µi vj , where the scalar α and the orthogonal unit vectors µ and ν are independent of the coordinate xi . Show that this velocity ﬁeld represents simple shearing. Find the principal values and directions of the rate of deformation D with respect to the directions of µ and ν. (28) Prove that, if the Dij components of a velocity ﬁeld are independent of the coordinates and the principal invariants ID and III D are both 0, the velocity ﬁeld represents simple shearing. (29) Consider the motion x1 = X1 + kX22 t2 ,

x2 = (1 + kt)X2 ,

and

x3 = X3

where k is a constant and the material coordinate XR designates the position of a particle at t = 0. (a) At t = 0 the corners of a unit square are at O (0, 0, 0), A (0, 1, 0), B (1, 1, 0), and C (1, 0, 0). Sketch the shape of the square at t = 1.5. (b) Obtain the spatial description of the velocity and acceleration ﬁelds. (c) Obtain the expressions for the rate of deformation D and the spin tensor W. (d) What happens to the volume of an inﬁnitesimal element located initially at (0.6, 0.5, 1)? (30) In the motion of a continuum, the velocity of a particle is given by v1 = (x12 + x1 x2 )e−kt ,

v2 = (x22 − x1 x2 )e−kt ,

v3 = 0

where k is a constant and t is time. Determine the following properties at point (1, 1, 1) when t = 0: (a) the principal values of the rate of deformation D, (b) the maximum shear rate. (31) For the motion of Problem (30), determine the volumetric strain-rate deﬁned by (1/dV)((D(dV))/Dt), where dV is the current volume of an element. (32) The velocity ﬁeld of a continuum is prescribed by v1 = f (x2 ) − x2 g(r),

v2 = x1 g(r),

v3 = 0

with r = (x12 + x22 )1/2

Determine the rate of deformation D and the vorticity vector w, which is the dual vector of the spin tensor W. Discuss the type of motion that the continuum is undergoing. (33) Let the components of D be

α [D] = β β

© 2005 by Chapman & Hall/CRC Press

β α β

β β α

140

Continuum Mechanics and Plasticity Consider a line element with direction denoted by the unit vector n. If the rate of extension of the line element is α, ﬁnd the condition that the components of n must fulﬁll.

(34) Consider the motion of a deformable element. Do all line elements in Figure 3.20 spin with the same angular velocity? The spin of which line element does the spin tensor W describe? x2

B

F

C G

A FIGURE 3.20

© 2005 by Chapman & Hall/CRC Press

D

x1

4 Conservation Laws and Constitutive Equation

4.1

Introduction

This chapter discusses the governing equations of a body undergoing deformation. The equations include the conservation laws of physics and the constitutive equations. The conservation laws of physics are the conservation of mass, linear momentum, angular momentum, and energy. These laws are ﬁrst developed in the global form and then reduced to the local form. The global form considers forces, momentum, or energy acted on the whole deformable body, whereas the local form refers to a generic inﬁnitesimal element of the body. The conservation laws are applicable to a body of any material. To distinguish between deformation of a body made of different materials, we need constitute equations. As an example, let us consider applying a tensile force to a long bar. The conservation laws for the problem are the same no matter what material the bar is made of. However, experiments show that long bars made of wood or steel will undergo different amounts of deformation when subjected to the same tensile force. Therefore, in order to accurately describe the elongation of the bars, we need to introduce constitutive equations, which accurately represent the two different materials of the bars, that is, we need a constitutive equation of for wood and another for steel. Constitutive equations are a set of equations, which describe the thermomechanical properties of a material. Depending on the simplicity/complexity of the material behavior that we wish to describe, we may need one constitutive equation or a set of constitutive equations. Hooke’s law is the most well-known constitutive equation for solids, and it is also the simplest form that a constitutive equation for solid can have. However, there is a limitation to the validity of Hooke’s law. It is usually applicable when the deformation is small and linearly elastic at room temperature. The equation needs to be modiﬁed or extended to a set of (nonlinear) equations when the deformation is large and nonelastic and not at constant temperature. Hooke’s law is also known as the stress–strain relation, because the equation relates the stress to the strain; for isotropic linearly elastic solid, it is 141

© 2005 by Chapman & Hall/CRC Press

142

Continuum Mechanics and Plasticity

written as σ = 2µε + λIεkk

(4.1)

where σ and ε are the engineering stress and strain, respectively, and µ and λ are the Lamé constants.‘ The effect of temperature on the material behavior is not discussed in this chapter. Even at constant temperature, the material behavior of a real material can be quite complex. Realistic constitutive equations should be used in order to obtain useful solutions of engineering problems. In addition to the elastic behavior, some materials exhibit strong viscous behaviors and some are signiﬁcantly inﬂuenced by plastic deformation. The viscous behaviors are observable in the forms of the strain-rate effect, creep and stress relaxation. These behaviors are usually discussed within the contest of viscoelasticity and viscoplasticity. The viscoplastic behavior is discussed in Chapter 5. The subject of plastic deformation is one of the main topics of this book and is thoroughly discussed in the later part of the book. In this chapter, we ﬁrst derive the conservation equations. The bulk material rate of change is discussed. This is useful in the derivation of the conservation laws in the global form. In the local form, we derive the conservation equations for an inﬁnitesimal material element at the deformed conﬁguration. This is a spatial description. We then discuss the material description of the conservation laws, which leads to the discussion of several stressmeasures, referring to the deformed or undeformed conﬁgurations. In the topics related to constitutive equations, we ﬁrst discuss the general principles, including the principle of material objectivity. We then derive the constitutive equation for large elastic deformation, which include different types of formulations. Emphasis is placed upon hyperelasticity and some examples are given. Finally, the generalized Hooke’s law for inﬁnitesimal elastic deformation is discussed.

4.2

Bulk Material Rate of Change

We discuss the bulk material rate here, because it is useful when we consider the global form of the conservation laws in the next section. The bulk material rate is the material rate of change of a physical property deﬁned over a material body. Referring to Figure 4.1, we let the material body occupy the space shown by the solid line at time t and let the body occupy the space shown by the dashed line at time t + t. The volume and surface of the body at t and t + t are (V, S) and (V , S ), respectively. Let φ(xi , t) be a property of the continuum, which is a tensor quantity. Considering the volume integral I= © 2005 by Chapman & Hall/CRC Press

V

φ dV

(4.2)

Conservation Laws and Constitutive Equation

143

∆V2 vdt S2 dS xi dS

vdt

n x3 x2

S1

xi + vi dt = xi + ∆xi n

V ⬘, S⬘ (at t + ∆t)

∆V1

V, S (at t) x1 FIGURE 4.1 Bulk material rate of change.

we are then interested in ﬁnding the derivative DI/Dt. To ﬁx ideas, let us assume that φ = ρ(xi , t) is the density of the continuum, then the integral I = V ρ dV is the total mass of the body. The derivative of (4.2) is

φ(xi + xi , t + t)dV − V φ(xi , t)dV] t [ V φ(xi , t + t)dV − V φ(xi , t)dV] = lim t→0 t [ V φ(xi + xi , t + t)dV − V φ(xi , t + t)dV] + lim t→0 t

[ DI = lim Dt t→0

V

(4.3)

In the second equality of (4.3), the term V φ(xi , t + t)dV has been added and subtracted. We now ﬁnd physical interpretations for the terms of (4.3). Letting V = υ + V1 , V = υ + V2 , then υ is the common volume of V and V and is denoted by the shaded area in Figure 4.1; V1 is the volume in V and V2 is the volume in V both of which are denoted by the moon-shaped area. Equation (4.3) may be interpreted as DI (Total mass in V at t + t − Total mass in V at t) = lim Dt t→0 t (Total mass in V at t + t − Total mass in V at t + t) + lim t→0 t = (Rate of increase of mass in ﬁxed region V) (Total mass in V2 at t + t − that in V1 at t + t) t→0 t

+ lim

© 2005 by Chapman & Hall/CRC Press

(4.4)

144

Continuum Mechanics and Plasticity

where the last term is the net amount of mass increased in V per unit time. Equation (4.3) may then be written as ( V2 φ dV − V1 φ dV) ∂φ dV + lim t→0 t V ∂t [ φvt · n dS + S1 φvt · (n dS)] ∂φ S2 = dV + lim t→0 t V ∂t

DI = Dt

(4.5)

Note that the surface S of the body at time t is seen in Figure 4.1 to be divided into S1 and S2 so that S = S1 + S2 . A particle on the surface S2 has coordinates xi with velocity v, and the particle moves to a new position xi + xi during the time interval t, and we write xi + vi t = xi + xi . Denoting the area element at this particle by dS and its unit normal by n, we observe that this area element sweeps through a volume V = vt · ndS during the time interval t, and area S2 sweeps through volume V2 . The same thing may be said of particles on surface S1 , except that the scalar product V = vt · ndS is negative. This may be seen from Figure 4.1, because vectors n and v form an obtuse angle. Thus, during time interval t, surface S1 sweeps through volume V1 . The two integrals within the parenthesis in (4.5) can then be added to form one integral and the equation becomes ∂φ ∂φ dV + φvi ni dS = dV + (φvi ),i dV V ∂t S V ∂t V ∂φ + φ,i vi + φvi,i dV = ∂t V

DI = Dt

(4.6)

The Gauss theorem discussed in Section 1.8.3 was used in the derivation of (4.6), which may be further written as D Dt

V

φ dV =

V

Dφ + φvi,i dV Dt

(4.7)

This is the material derivative of the integral of a property φ deﬁned over volume V. We used φ = ρ in the above derivation for easy interpretation, but (4.7) is valid for any scalar property of the material. We now consider an alternative derivation of (4.7). Let I = I(t) which, in general, is a function of time and we write I=

V

φ dV =

V0

φ(XR , t) det F dV0

(4.8)

In arriving at the last equality of (4.8), (3.82) and the coordinate transformation XR = XR (xi , t) was applied. Noting that V0 is time independent, we

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation differentiate (4.8) to obtain DI Dφ D = det F + φ (det F) dV0 Dt Dt V0 Dt

145

(4.9)

To further reduce equation (4.9) to a simple form, we apply the following expression that was deduced in Example 3.9 DJ ∂vk =J Dt ∂xk

(4.10)

Note that J = det F. Using (4.10), (4.9) becomes DI = Dt

V0

Dφ Dφ det F + φ det F vi,i dV0 = + φvi,i det F dV0 (4.11) Dt V0 Dt

Therefore, we may conclude that DI = Dt

V

Dφ + φvi,i dV Dt

(4.12)

which is the same as (4.7).

4.3

Conservation Laws

There are three conservation laws from physics, and they are valid for all materials. They are: (i) the conservation of mass, (ii) the conservation of momentum, and (iii) the conservation of energy. These laws are discussed individually and written in mathematical expressions in this section.

4.3.1

The Conservation of Mass

The mass of a body is preserved when only thermo-mechanical behavior is being considered. In this case, the rate of change of mass is zero. Setting φ = ρ in (4.2), the integral I is the mass of the body. The global form of the conservation of mass is written as D ρ dV = 0 (4.13) Dt V Using (4.7), (4.13) may be further written as D Dt

© 2005 by Chapman & Hall/CRC Press

V

ρ dV = 0 =

V

Dρ + ρvi,i dV Dt

(4.14)

146

Continuum Mechanics and Plasticity

which must be true for all volume elements. Thus, the local form (or differential form) of the conservation of mass is Dρ + ρvi,i = 0 Dt

(4.15)

Dρ ∂ρ(xi , t) ∂ρ vj = + Dt ∂t ∂xj

(4.16)

∂(ρvi ) ∂ρ =0 + ∂t ∂xi

(4.17)

But, since

we obtain from (4.15)

Equation (4.17) is known as the continuity equation in ﬂuid mechanics.

4.3.2

The Conservation of Momentum

We need to consider both the conservation of linear momentum and angular momentum. The rate of change of linear momentum is equal to the resultant force and the conservation equation is D Dt

V

ρvi dV =

V

bi dV +

(n)

S

ti

dS

(4.18)

Equation (4.18) is the conservation of linear momentum in the global form. The left-hand side of (4.18) is the rate of change of linear momentum. The ﬁrst term on the right-hand side is the total body force and the second term is the total surface traction. Using (2.8) and an identity proven in Example 4.1, (4.18) may be written as

D bi dV + σki nk dS = Dt V S

V

ρvi dV =

V

ρ

Dvi dV Dt

(4.19)

or, by use of the Gauss theorem, we obtain V

bi + σki,k − ρ

Dvi Dt

dV = 0

(4.20)

In the local form, (4.20) reduces to σki,k + bi = ρ which is known as the equation of motion.

© 2005 by Chapman & Hall/CRC Press

Dvi Dt

(4.21)

Conservation Laws and Constitutive Equation

147

The conservation of angular momentum states that the rate of change of the angular momentum is equal to the sum of moments of forces acting on the body. This law leads to the symmetry of stress tensor and has been discussed in Section 2.6 for the case when material element is in equilibrium. In the case of material element in motion, we have D (n) ρeijk xi bj dV + eijk xi tj dS = ρeijk xi vj dV (4.22) Dt V V S The ﬁrst term on the left-hand side of (4.22) denotes the moment due to the body force, the second term denotes the moment due to surface traction, and the term on the right-hand side denotes the rate of change of the angular momentum. Using (2.8) and the Gauss theorem, (4.22) is written as V

ρeijk xi bj +

D ∂ (eijk xi σmj ) dV = ρeijk (xi vj ) dV ∂xm Dt V Dvj = ρeijk vi vj + xi dV Dt V

(4.23)

in which ρeijk vi vj = 0. Hence, Dvj eijk xi σmj,m + bj − ρ dV + eijk σji dV = 0 Dt V V

(4.24)

By use of the equation of motion (4.21), the ﬁrst integral of (4.24) vanishes, and therefore, eijk σij = 0

(4.25)

σij = σji

(4.26)

which leads to

using an argument similar to that used in Section 2.6. Thus, we have shown that the conservation of angular momentum leads to the symmetry of the stress tensor for a body in motion. EXAMPLE 4.1 Show that D/Dt V ρφ dV = V ρ(Dφ/Dt) dV, where φ is a physical property deﬁned in V. Proof From (5.7), we have D D Dρ Dφ (ρφ)dV = (φρ) + φρvi,i dV = + ρvi,i + ρ dV φ Dt Dt Dt Dt V (a)

© 2005 by Chapman & Hall/CRC Press

148

Continuum Mechanics and Plasticity

In the last equality, Dρ/Dt + ρvi,i = 0 due to conservation of mass. Hence, (a) reduces to D Dt

4.3.3

V

ρφ dV =

V

ρ

Dφ dV Dt

(b)

The Conservation of Energy

The law of conservation of energy is the ﬁrst law of thermodynamics. According to this law, the sum of material derivatives of the internal and kinetic energies is equal to the sum of the rate of work of body and surface forces plus all other energies that enter the body per unit time. Other energies may include thermal, electrical, magnetic, or chemical energies. In this elementary text, we consider only the thermal energies and write DE DK DW DQ + = + Dt Dt Dt Dt

(4.27)

The equation is now explained term by term. E denotes the internal energy of the material element and is an extensive quantity, that is, an internal energy density ε may be deﬁned either per unit volume or per unit mass. In the case that ε is deﬁned per unit mass, we write E=

V

ρε dV

(4.28)

An extensive quantity is doubled if the mass or volume is doubled. On the other hand, the density cannot be deﬁned for an intensive quantity. Examples of intensive quantities are temperature and pressure. The internal energy includes all forms of energy in a system other than kinetic energy and potential energy. It represents energy modes on the microscopic level such as energy associated with nuclear spin, molecular binding, molecular translation and rotation, and molecular vibration, etc. The kinetic energy is related to the motion of the macroscopic element and is written as 1 K= ρvi vi dV (4.29) 2 V The second term in (4.27) is the rate of change of the kinetic energy and the third term is the rate of work due to external forces and is written as DW (n) = bi vi dV + ti vi dS (4.30) Dt V S and the last term of (4.27) is the rate of heat supply.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

149

There are two categories of heat supply: the heat ﬂowing across the boundary and the heat source. The heat ﬂowing through area element dS is −hi ni dS, where hi is the heat ﬂux vector and the direction of hi is the direction of the heat ﬂow. The magnitude of hi is the amount of heat per unit time per unit area normal to thedirection of heat ﬂow. Therefore, the part of DQ/Dt due to conduction is − S hi ni dS. We note that heat ﬂowing into the volume element is considered positive. Since the angle between hi and ni is obtuse, the negative sign is needed to make the heat ﬂow positive. The part of DQ/Dt due to distributed heat sources is D/Dt V ρq dV; where q is the heat supply per unit mass. Hence, the equation of conservation of energy in the global form, (4.27), may be written as D Dt

1 D ρε dV + ρvi vi dV Dt V V 2 D (n) = bi vi dV + ti vi dS − hi ni dS + ρq dV Dt V V S S

(4.31)

Using the result of Example 4.1, (4.31) becomes Dvi Dε ρvi dV + dV Dt Dt V V Dq = (σki vi ),k dV + bi vi dV − hi,i dV + ρ dV V V V V Dt

ρ

(4.32)

The ﬁrst integral on the right-hand side of (4.32) is

V

(σki vi ),k dV =

V

(σki,k vi + σki vi,k ) dV

(4.33)

Then, by use of the equation of motion (4.21), the energy balance equation may be simpliﬁed. Hence, (4.32) reduces to ρ

Dq Dq Dε = σki vi,k − hi,i + ρ = σki Dik − hi,i + ρ Dt Dt Dt

(4.34)

This is the local form of the ﬁrst law of thermodynamics for a continuous medium. Note that no kinetic energy term appears in the local form of the ﬁrst law, since it gets canceled out by the rate of work done. Some remarks are in order. The conservation laws derived in this section apply to all materials whether they are ﬂuid or solid, dissipative or elastic (conservative). In particular, the ﬁrst law as derived applies to all materials as well as processes reversible or irreversible. The validity of these equations

© 2005 by Chapman & Hall/CRC Press

150

Continuum Mechanics and Plasticity

is subject to the constraint of a one-to-one and onto transformation which excludes: (a) diffusion processes; (b) chemical effects such as reactions and phase changes; (c) electromagnetic phenomena; and (d) polar media, that is, materials with distributed surface and body moments whose deformation requires account of local rotation and higher order deformation gradients. To address these sophisticated behaviors, the equations would have to be modiﬁed. Nevertheless, the equations in this section provide the foundations for further studies.

4.4

The Constitutive Laws in the Material Description

The local form of conservation laws of Section 4.3 is written based on an inﬁnitesimal material element at the deformed conﬁguration. In particular, the forces are applied to the element at the deformed conﬁguration. In the study of continuum mechanics undergoing large deformation, it is necessary to distinguish between quantities that have been deﬁned with reference to the deformed conﬁguration and those that have been deﬁned with reference to the reference conﬁguration. The former is used in the spatial description of the conservation laws and the latter the material description. It is preferable by some investigators to use one description for solving certain problems and use the other description for other types of problems. The decision is based on the material properties and boundary conditions of the problems. We like to emphasize that, in the material description of conservation laws, the forces are still applied to the element at the deformed conﬁguration, but some quantities as deﬁned are referred to the reference conﬁguration. In this section, we discuss the material description of the constitutive laws.

4.4.1

The Conservation of Mass

The conservation of mass is expressed as dm = ρ0 dV0 = ρ dV

(4.35)

which, from (3.82), may also be written as ρ0 dV = det(F) = J = dV0 ρ

(4.36)

ρ0 = ρ det(F)

(4.37)

or

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

151

This is a form of the conservation of mass and it may also be written as D (ρ det F) = 0 Dt

4.4.2

(4.38)

The Conservation of Momentum

We ﬁrst discuss different stress measures referred to either deformed or undeformed conﬁgurations and then express the conservation of momentum using these stress measures. 4.4.2.1 The Piola–Kirchhoff stress tensors The stress tensor σij that we have been using so far is called the Cauchy stress and it is deﬁned based on a deformed element using the spatial description. The components of σ refer to a Cartesian coordinate system. Sometimes it is desirable to deﬁne stress measures that refer to the undeformed or reference conﬁguration. In this section, we discuss two such stress measures known as the ﬁrst and second Piola–Kirchhoff stresses (or the 1st P–K and 2nd P–K stresses for short). In the instantaneous state (at time t), the inﬁnitesimal force dPi transmitted in the surface element dai is given by (n)

dpi = ti

da = σji nj da = σji daj

or

dp = σT · n da

(4.39)

(0)

For the same inﬁnitesimal force, we may deﬁne a stress vector ti and a stress (0) tensor TRi as in the following expressions. Both new stress vector and stress tensor refer to the initial state. Thus, (0)

(0)

(0)

dpi = ti dA = TRi NR dA = TRi dAR

or (n)

dp = (T(0) )T · N dA

(4.40)

(0)

By comparing (4.39) and (4.40), we see that ti and ti act in the same direction (0) but are different in magnitude. TRi is called the Lagrangian stress, or the 1st P–K stress, and it is also known as the nominal stress. By use of the Nanson’s formula (3.92), we may combine (4.39) and (4.40) to obtain dpi = σji daj = σji J

∂XR (0) dAR = TRi dAR ∂xj

(4.41)

From the last two expressions of (4.41), we ﬁnd the relation between T(0) and σ as (0)

TRi = Jσji

© 2005 by Chapman & Hall/CRC Press

∂XR ∂xj

or

T(0) = JF−1 · σ

(4.42)

152

Continuum Mechanics and Plasticity ti(0)

(0) T13

ti(n) ni (0)

da (0) T11

T12

dA 3 NR(1, 0, 0) 2 1 FIGURE 4.2 First P–K stresses.

With the help of tensor bases, (4.42) may be written as (0)

∂XR eR ⊗ ei · (σmn em ⊗ en ) ∂xi ∂XR ∂XR σmn (eR ⊗ ei ) · (em ⊗ en ) = J =J σmn (ei · em ) · (eR ⊗ en ) ∂xi ∂xi ∂XR ∂XR σin eR ⊗ en = Jσji eR ⊗ e i (4.43) =J ∂xi ∂xj

TRi eR ⊗ ei = J

The components of (4.43) lead to the ﬁrst expression of (4.42). It is useful (0) at this point to illustrate the physical signiﬁcance of the components TRi of the 1st P–K stress. Consider area element dA with a normal NR = [1, 0, 0]. (n) This area is deformed into da with a normal ni . The stress vectors ti and (0) ti for this case are shown in Figure 4.2. They have the same direction but dif(0) ferent magnitudes. The stress vector ti is then decomposed into components (0) (0) (0) T11 , T12 , and T13 with respect to the xi coordinate system. Using a similar (0) procedure, we can consider an area with normal NR [0, 1, 0] to deﬁne T21 , (0) (0) (0) (0) (0) T22 , and T23 ; and a similar approach is used to deﬁne T31 , T32 , and T33 . (0) (0) Note that σij is symmetric, but, from (4.42), TRi is not. Since TRi is not symmetric, this tensor is difﬁcult to use in constitutive equations that are to represent the stress components in terms of the components of the symmetric strain tensor. This difﬁculty can be avoided by deﬁning a symmetric stress called the Piola–Kirchhoff stress (or the 2nd P–K stress), which is now explained. Before the inﬁnitesimal force dpj transmitted in the deformed conﬁguration is referred to the surface element in the reference conﬁguration, let it be subjected to the same transformation that changes the deformed side dxi of the surface element da into the corresponding initial side dXR of dA. That is, we

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

153

~ dp R dpi

NR

dAR XR

dai

ni

xi

V

V0

Rt

R0 FIGURE 4.3 The ﬁctitious force d˜pR .

introduce a ﬁctitious force (or the pseudo-force) d˜pR such that d˜pR =

∂XR dpj ∂xj

(4.44)

which follows the same transformation as in dXR =

∂XR dxj ∂xj

(4.45)

In this operation, the external loading is transformed back to the material description ﬁrst, and the 2nd P–K stress is then deﬁned per unit undeformed area. The ﬁctitious force d˜pR and the initial area dAR have been stretched and rotated the same amount relative to the ﬁnal position dpi and dai , respectively. This deﬁnition of d˜pR is illustrated in Figure 4.3. Using this ﬁctitious force we now deﬁne the 2nd P–K stress tensor RS which refers to the initial area dAR and the relation is d˜pR = SR NS dA = SR dAS

or

dp˜ = · N dA

(4.46)

Note that the form of (4.46) is similar to that of (4.40). We now proceed to determine the relation between RS and σij . Substituting (4.39) into (4.44), we have d˜pR =

∂XR ∂XR ∂XS σkj dak = σkj J dAS ∂xj ∂xj ∂xk

(4.47)

Comparing (4.46) and (4.47), we obtain

RS = Jσjk

© 2005 by Chapman & Hall/CRC Press

∂XR ∂XS ∂xj ∂xk

or

(0) ∂XS

RS = TRi

∂xi

(4.48)

154

Continuum Mechanics and Plasticity

It is then easy to show that (0)

TRi = RS

∂xi ∂XS

(4.49)

(0)

which is the relation between TRi and RS . In the symbolic notation, the above relations may be written as = JF−1 · σ · F−T

and

= T(0) · F−T

where F−T = (F−1 )T

(4.50)

Using the tensor bases, the 2nd P–K stress is written as = RS eR ⊗ eS

(4.51)

Various stress measures are further discussed in Chapter 11 referring to curvilinear coordinates. For the problem of simple shearing, if the XR and the xi systems coincide, that is, the 1-axis is horizontal and the 2-axis vertical, discuss the (0) (0) directions of TRi and ﬁnd the equations relating TRi to the Cauchy stress σij (0) (note that both σij and TRi are Cartesian components). EXAMPLE 4.2

Solution Figure 4.4 shows that a square element is deformed into a parallelogram by simple shearing. The initial areas for Face 1 and Face 2 of the square element are dA(1) and dA(2) and they are deformed into da(1) and da(2) , respectively. (1) (2) The unit normal to the areas are NR and NR and they are deformed into (1) (2) ni and ni , respectively. We now consider the forces and stress components acting on the two faces of the element. (1)

(1)

On face 1: The unit normals are NR = [1, 0] and ni = [cos γ , − sin γ ], where γ is the shearing angle of the element shown in Figure 4.4. The initial and deformed areas are related by da(1) cos γ = dA(1)

(a)

Using (4.39), the inﬁnitesimal force acting on this face is (1)

dpi

(n)1

= ti

(1)

(1)

(1)

da(1) = σji nj da(1) = (σ1i n1 + σ2i n2 ) da(1)

(b)

On the other hand, the same force may be expressed in terms of (4.40) as (1)

dpi

(0)1

= ti

© 2005 by Chapman & Hall/CRC Press

(0)

(1)

(0)

dA(1) = TRi NR dA(1) = T1i dA(1)

(c)

Conservation Laws and Constitutive Equation

155

NR(2) ti(0)2

(0)

T22

(0)

ni(2)

ti(0)1

T21

dA(2)

(0)

T12

ti(n)2

NR(1)

(0)

T11

22

(1)

21

dA

da(2) 2

ti(n)1

12

11

1

ni(1)

da(1)

FIGURE 4.4 Stress components in simple shearing.

By comparing (b) and (c), we obtain (1)

(1)

(0)

(σ1i n1 + σ2i n2 ) da(1) = T1i dA(1)

(d)

which, by use of (a), may be simpliﬁed to yield (0)

σ1i cos γ + σ2i (− sin γ ) = T1i cos γ

(e)

From (e), we obtain (0)

T11 = σ11 − σ21 tan γ

and

(0)

T12 = σ12 − σ22 tan γ

(2)

(f)

(2)

On face 2: The unit normals are NR = [0, 1] and nR = [0, 1], and the area does not change, so that da(2) = dA(2) . Following the same procedure as in Face 1, we ﬁnd (2)

(n)2

= ti

dpi (2)

dpi

(0)2

= ti

(2)

(2)

da(2) = σji nj da(2) = σ2i n2 da(2) = σ2i da(2) (0)

(2)

(0)

(2)

(0)

dA(2) = TRi NR dA(2) = T2i N2 dA(2) = T2i dA(2)

(g) (h)

From (g) and (h), we obtain (0)

(0)

σ2i da(2) = T2i dA(2) = T2i da(2)

with dA(2) = da(2)

(i)

Therefore, we ﬁnd (0)

σ2i = T2i , © 2005 by Chapman & Hall/CRC Press

(0)

σ21 = T21 ,

(0)

σ22 = T22

(j)

156

Continuum Mechanics and Plasticity

We now summarize the stress components found from (f ) and (j) as (0)

(0)

T11 = σ11 − σ21 tan γ , (0)

T21 = σ21 = σ12

and

T22 = σ22 , (0)

(0)

T12 = σ12 − σ22 tan γ

(0)

T12 = T21

(k)

We remark that on Face 1, the normal n(1) is not in the direction of any xi axis. The stress vector t(n)1 is further related to vectors ti , by use of (2.6), acting on cross-sections of the material element that are parallel to the coordinate planes of the xi system, and the vectors ti further deﬁne the components of the Cauchy stress. On the other hand, since N(1) is in the direction of X1 , t(0)1 is already acting on a plane parallel to a coordinate plane, and, therefore, its (0) components with respect to the xi system deﬁne the TRi stress. EXAMPLE 4.3

Find the stress components of Example 4.2 using (4.42).

Solution From (3.20), the simple shear may be described by x1 = X1 + X2 tan γ ,

x2 = X2

(a)

with J = |F| = 1

(b)

The deformation gradient is

1 tan γ 0 1

[F] =

From (4.42), we write σij = J −1

∂xi (0) (0) T = FiR TRj ∂XR Rj

(c)

The components are (0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

σ11 = F1R TR1 = F11 T11 + F12 T21 = T11 + T21 tan γ σ12 = F1R TR2 = F11 T12 + F12 T22 = T12 + T22 tan γ (0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

σ21 = F2R TR1 = F21 T11 + F22 T21 = T21 σ22 = F2R TR2 = F21 T12 + F22 T22 = T22

These results are the same as those obtained in Example 4.2.

© 2005 by Chapman & Hall/CRC Press

(d) (e) (f) (g)

Conservation Laws and Constitutive Equation

157

For the problem of simple shearing discussed in Example 4.2, ﬁnd the components of the 2nd P–K stress RS .

EXAMPLE 4.4

Solution Using the expression for F found in Example 4.3 and noting that J = |F| = 1, we ﬁnd −1

[F]

∂XS 1 = = 0 ∂xk

− tan γ 1

(a)

From (4.50) we have (0) ∂XS

RS = TRi

(b)

∂xi

Using (a), (b) reduces to (0) (0) T11 − T12 tan γ [ ] = (0) (0) T21 − T22 tan γ

(0)

T12

(0) T22

(c)

Using (k) of Example 4.2, we obtain from (c) (0)

(0)

11 = T11 − T12 tan γ = σ11 − 2σ12 tan γ + σ22 tan2 γ (0)

12 = T12 = σ12 − σ22 tan γ (0)

(d)

(0)

21 = T21 − T22 tan γ = σ12 − σ22 tan γ = 12 (0)

22 = T22 = σ22 In the case of uniform extension along the 1-direction, the applied tensile force is P, shown in Figure 4.5(a); the initial dimensions of the rectangular bar are X1 × X2 × X3 with cross-sectional area A; and the current dimensions are x1 × x2 × x3 with cross-sectional area a. Find the components of σ, T(0) , and . EXAMPLE 4.5

Solution Consider the deformation x1 = λ1 X1 ,

© 2005 by Chapman & Hall/CRC Press

x2 = λ2 X2 ,

x3 = λ3 X3

(a)

158

Continuum Mechanics and Plasticity (a)

2

P

P

(b)

1

2 P

1

P FIGURE 4.5 Effect of rotation on stress components.

The deformation gradient is

λ1 [F] = 0 0

0 λ2 0

0 0 λ3

1 λ1 −1 [F ] = 0 0

0 1 λ2 0

0

0 1 λ3

(b)

and J = det F = λ1 λ2 λ3 . The components of the Cauchy stress are σ11 =

P , a

other components = 0

(c)

The components of the 1st P–K stress may be found from (4.42) in the matrix form as [T (0) ] = J[F−1 ][σ ]

© 2005 by Chapman & Hall/CRC Press

(d)

Conservation Laws and Constitutive Equation

159

and the components of the 2nd P–K stress may be found from (4.50) in the matrix form as [ ] = J[F−1 ][σ ][F−T ]

(e)

Substituting the above information into (d) and (e) and performing the matrix multiplications, we obtain σ

11

λ1 (0) TRi = (λ1 λ2 λ3 ) 0 0

σ

0 0 0

0

, 0 0

RS = (λ1 λ2 λ3 )

11 λ21

0

0 0

0 0

0

0 0

(f)

The nonzero term of T (0) is (0)

T11 = λ2 λ3 σ11 =

x2 x3 a a σ11 = σ11 = X2 X3 A A

P P = a A

(0)

It is seen that T11 is the nominal stress, that is, force over initial area, but σ11 is the true stress. This physical interpretation of T(0) is good only for deformation that does not involve rotation. In the case of simple shear, as discussed in Example 4.2, no such assertion can be made about the 1st P–K stress. The nonzero component of RS is

11 = (λ1 λ2 λ3 )

σ11 λ21

=

λ2 λ3 a σ11 aP 1 1 σ11 = = = λ1 A λ1 A a λ1 λ1

P A

(g)

We see from (g) that no clear physical meaning can be associated with 11 . However, from (4.44), the ﬁctitious force is

1 λ1 −1 [d˜p] = [F ][dp] = 0 0

0 1 λ2 0

0 P P λ1 0 0 =0 0 1 0

(h)

λ3

Thus, (g) may be written as

11 =

d˜p11 A

(i)

It is the component of the ﬁctitious force [d˜p] in the X1 direction divided by the initial cross-sectional area A.

© 2005 by Chapman & Hall/CRC Press

160

Continuum Mechanics and Plasticity

EXAMPLE 4.6 Referring to Example 4.5 and Figure 4.5(b), if, after the stretch, the specimen is rotated 90◦ counterclockwise and the traction P also rotates with it, determine the expressions for the Cauchy stress, the 1st P–K stress, and the 2nd P–K stress components after rotation and thereafter discuss the physical meaning of the three stress tensors.

Solution Let us call the initial stretching of the specimen discussed in Example 4.5 stage 1, and the quantities of this stage are denoted by

λ1 [F(1) ] = 0 0

0 0 λ3

0 λ2 0

σ

0 0

11 λ21

0

0

0 0

0 0

λ1 [T 0(1) ] = (λ1 λ2 λ3 ) 0 0 σ

0

0

0 0 0

P A = 0 0 0 0

11

[ (1) ] = (λ1 λ2 λ3 )

P a [σ (1) ] = 0 0

0 0 0 0 0 0

0 0 0

P Aλ1 = 0 0 0 0

(a)

0

0 0 0 0 0

We now apply a rotation Q to various tensors to obtain the quantities of the second stage denoted by F(2) = Q · F(1) ,

σ(2) = Q · σ(1) · QT

T0(2) = J[F(2) ]−1 · σ(2) = J[F(1) ]−1 · Q−1 · Q · σ(1) · QT = J[F(1) ]−1 · σ(1) = T0(1) · QT (2) = T0(2) · [F(2) ]−T = T0(1) · QT · [[F(1) ]−1 · Q−1 ]T = T0(1) · QT · [Q−1 ]T · [F(1) ]−T = T0(1) · [Q−1 · Q]T · [F(1) ]−T = T0(1) · [F(1) ]−T = (1)

(b)

It is seen from (b) that under a rotation Q, the Cauchy stress σ transforms like a second-rank tensor; the 1st P–K stress transforms like a ﬁrst-rank tensor; and the 2nd P–K stress transforms like a tensor of rank zero.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

161

For this example, the rotation is

0 [Q] = 1 0

−1 0 0

0 0 1

(c)

Using (c) in (b), the stresses in stage 2 are [σ (2) ] = [Q][σ (1) ][Q]T

0 −1 = 1 0 0 0

P 0 a 0 0 1 0

0 0 0

0 0 −1 0 0 0

0

1 0 0 0 = 0 0 1 0

0 0 1 0 0 −1 0 0 = 0 0 0 0 0 1 0 0 0 P 0 0 Aλ1 [ (2) ] = [ (1) ] = 0 0 0 0 0 0

P A [T 0(2) ] = [T 0(1) ][Q]T = 0 0

0

0 P a 0

0 0 0

P A 0 0

0 0 0

(d)

(e)

(f)

We see from (d) that the Cauchy stress has a nonzero component in (2)

σ22 =

P a

(g)

which still lives up to the interpretation of true stress even after the rotation. From (e), we see that the 1st P–K stress has only one nonzero component in 0(2)

T12 =

P , A

0(2)

other TRi = 0

(h)

The second subscript i = 2 indicates that the force P is in the 2-direction, while the ﬁrst subscript R = 1 indicates that this 1st P–K stress component lies on an undeformed area with normal N = [1, 0, 0]. This nonzero component is, therefore, a shear stress and it indicates that the interpretation of nominal stress is no longer appropriate, since a normal stress turns into a shear stress due to rotation. We see from (f) that the 2nd P–K stress does not change due to the imposed rotation. A normal stress before rotation remains a normal stress and a shear stress before rotation remains a shear stress. It is useful from computational viewpoint to deﬁne the 2nd P–K stress, because it is symmetric, it does not change due to imposed rotation, and it is the energy conjugate of Lagrangian

© 2005 by Chapman & Hall/CRC Press

162

Continuum Mechanics and Plasticity

strain E (the concept of work conjugate will be discussed in Section 4.4.3). We note, however, that the physical meaning of the 2nd P–K stress is not clear. In equation (i) of Example 4.5, the 11 component of this stress is the ﬁctitious force divided by initial area A. The ﬁctitious force d˜pR involves stretching and rotation of dpi and, therefore, the 2nd P–K stress does not have the physical meaning of a pure stress. For this reason the 2nd P–K stress should not be used to deﬁne the yield criterion, the fracture criterion, or to set up material instability conditions. 4.4.2.2 Conservation of momentum From (4.39) and (4.40) we have (n)

ti

(0)

da = σji nj da = TRi NR dA

(4.52)

Integrating (4.52) over the surface of the body, we write

S

σij ni da =

S0

(0)

TRi NR dA =

(0)

∂TRi dV0 ∂XR

V0

(4.53)

Let Bi be the body force per unit volume of the undeformed body, we then write Bi dV0 = bi dV

or

Bi = bi

dV = bi J dV0

(4.54)

Integrating (4.54) over the undeformed volume of the body, the resulting total body force is V0

Bi dV0

(4.55)

We note that in the above equations, the forces are applied to the deformed body, although the integrals are over the undeformed body V0 . The momentum is also referred to the deformed body V at time t, and the rate of change of linear momentum is D Dt

V

ρvi dV =

D Dt

V0

ρ0 vi dV0 =

V0

ρ0

Dvi dV0 Dt

(4.56)

Using (4.53), (4.55) and (4.56), the conservation of linear momentum is now

Dvi ρ0 dV0 = Dt V0

© 2005 by Chapman & Hall/CRC Press

V0

(0)

∂TRi dV0 + ∂XR

V0

Bi dV0

(4.57)

Conservation Laws and Constitutive Equation

163

which leads to the following equation of motion in the material description (0)

∂TRi Dvi + Bi = ρ0 ∂XR Dt

(4.58)

In terms of the 2nd P–K stress, the equation of motion becomes ∂ ∂XR

4.4.3

∂xi

RS ∂XS

+ Bi = ρ0

Dvi Dt

(4.59)

The Conservation of Energy

The spatial description for the conservation of energy is given in (4.31). Referring to the undeformed state, this equation can be written as D Dt

1 D ρ0 vi vi dV0 Dt V0 V0 2 D (0) = Bi vi dV0 + TRi NR vi dS0 − hR NR dS0 + ρ0 q dV0 Dt V0 V0 S0 S0 ρ0 ε dV0 +

(4.60) where hR is the component of the heat ﬂux vector referring to the material coordinates, so that hR = (∂XR /∂xi )hi . The energy balance equation (4.60) further becomes Dε Dvi ρ0 ρ0 vi dV0 + dV0 Dt Dt V0 V0 (0) ∂TRi (0) ∂vi vi dV0 = Bi vi dV0 + + TRi ∂XR ∂XR V0 V0 ∂hR Dq − dV0 + ρ0 (4.61) dV0 Dt V0 ∂XR V0 Three terms in the above equation cancel out due to the equation of motion (4.58). We then obtain V0

Dε Dq ∂hR (0) ∂vi ρ0 − TRi dV0 = 0 + − ρ0 Dt ∂XR ∂XR Dt

(4.62)

which leads to the conservation of energy in the local form as ρ0

© 2005 by Chapman & Hall/CRC Press

Dε Dq ∂hR (0) ∂vi = TRi − + ρ0 Dt ∂XR ∂XR Dt

(4.63)

164

Continuum Mechanics and Plasticity

The rate of work term on the right-hand side of (4.63) should be discussed further. This term represents part of work rate that affects the strain energy of a material element (the idea of strain energy is discussed in the later sections of this chapter). This term is sometimes called the speciﬁc rate of work per ˙ is obtained unit mass or the stress power. In this term, the rate of work w using the 1st P–K stress, which may be expressed in terms of the 2nd P–K stress using (4.49). Thus, (0)

TRi

(0)

TRi

∂vi (0) ∂ = TRi ∂XR ∂XR

Dxi Dt

(0)

= TRi

D Dt

∂xi ∂XR

(0) DFiR

= TRi

Dt

(4.64)

∂vi ∂xi ∂vi ∂xi ∂vi ∂xr = RS = RS ∂XR ∂XS ∂XR ∂XS ∂xr ∂XR 1 ∂vi ∂xi ∂xr ∂xi ∂xr DERS ∂vr

RS = RS = + = RS Dir 2 ∂xr ∂xi ∂XS ∂XR ∂XS ∂XR Dt (4.65)

˙ may Equation (3.200) was used in the last expression of (4.65). In addition, w also be expressed in terms of the Cauchy stress. Using (4.42), we write (0)

TRi

∂vi ρ0 ∂XR ∂vi ρ0 ∂vi ρ0 = σji = σji = σji Dij ∂XR ρ ∂xj ∂XR ρ ∂xj ρ

(4.66)

We conclude from (4.64 to 4.66) that the speciﬁc rate of work per unit mass may be written as ˙ = w

1 1 (0) DFiR 1 DERS σij Dij = TRi = RS ρ ρ0 Dt ρ0 Dt

(4.67)

We have thus found three pairs of work (or energy) conjugates. They are σ and D, T(0) and F, and and E. The conjugate stress and strain should be used in any formulation of continuum mechanics problems. Using (4.67), the energy balance equation can also be written as ρ0

4.5

Dε DERS Dq ∂hR + ρ0 = RS − Dt Dt ∂XR Dt

(4.68)

Objective Tensors

Only objective tensors are used to formulate the constitutive equations. Objectivity is also known as reference frame indifference. Tensor quantities that depend only on the orientation of the spatial reference frame, which is given by Q, and not on the other aspects of the motion of the reference frame

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

165

(e.g., translation, velocity and acceleration, angular velocity and angular acceleration) are said to be indifferent, or objective. Consider two observers each having his/her own reference frame. Components of a tensor observed by two different observers are different. This difference is due to the different orientations of the observers but not to relative motions between the observers. In this contest, we are not talking about the change of coordinate system (each observer is free to choose a coordinate system), but are concerned with the change of observer positions and orientations, or the change of reference frame. Therefore, in the discussion of objectivity, transformation of coordinate system does not play any part. The reference frame of an observer may be conveniently denoted by (o, x), where x is a spatial coordinate system with origin O. We may imagine that one observer is attached to the continuous body and moves with the body and the other observer is stationary. Then, the two reference frames attached to the two observers are differed by a translation of the origin and a rotation of orientation. In the general case, both observers may not be stationary. Let us introduce two reference frames (o, x) and (o, ¯ x¯ ) as shown in Figure 4.6. Consider a particle P in the body. The position vector of the particle in (o, ¯ x¯ ) at time t is x¯ and that of the same particle in (o, x) at time t is x. The latter vector is seen by an observer sitting in (o, ¯ x¯ ) as QT · x. These position vectors are thus related by x¯ = c(t) + QT · x

x¯ i = ci + Qji xj

or

(4.69)

where c is the position vector of o in (o, ¯ x¯ ) and Q is an orthogonal tensor that gives the orientation of (o, x) relative to (o, ¯ x¯ ). Thus, (o, x) is different from (o, ¯ x¯ ) by a rigid-body translation c and a rotation Q. Deﬁniton of objective tensors A scalar f , a vector v, and a second-rank tensor T are objective, if for reference frames (o, ¯ x¯ ) and (o, x), related by (4.69), the corresponding scalar f¯, vector v, ¯

P

–

3

3

QT. x

x– o– –

1 FIGURE 4.6 Rotation of reference frames.

© 2005 by Chapman & Hall/CRC Press

o

c –

2

R

1

2

166

Continuum Mechanics and Plasticity

and tensor T¯ are related by f¯ = f

(scalar)

v¯ = QT · v

or

v¯ i = Qji vj

T¯ = QT · T · Q

or

T¯ ij = Qri Qsj Trs

(4.70) (vector) (tensor)

(4.71) (4.72)

We note that a rotation of the body is equivalent to the rotation of the reference frame of the same magnitude but in opposite direction (see Section 1.6). Therefore, if we consider a rigid rotation of the body with ﬁxed reference frame, then (4.69) to (4.72) become x¯ = c(t) + Q · x f¯ = f v¯ = Q · v

(scalar) (vector)

T¯ = Q · T · QT

(tensor)

(4.73) (4.74) (4.75) (4.76)

Either (4.69)–(4.72) or (4.73)–(4.76) may be used to deﬁne objectivity. Since the objectivity should be valid for any rotation Q, we shall make no effort to specify the sense of rotation, when the objectivity of a quantity is being investigated.

4.6

Property of Deformation and Motion Tensors Under Reference Frame Transformation

We investigate the transformation property of tensors F, C, B, v, L, D, and W. Using (4.69), the transformation equation for FiR is ∂ x¯ i ∂ x¯ i ∂xk ∂xk = = Qki (t) = Qki FkR F¯ iR = ∂XR ∂xk ∂XR ∂XR

(4.77)

which may be written in the matrix form as ¯ = [Q]T [F] [F]

(4.78)

that is, F behaves like a vector in a rotation QT of the body or a rotation Q of the spatial reference frame. Note that since Q is arbitrary, we can use either Q or QT in the discussion of objectivity. Even though F is a second-rank tensor, it transforms as a vector in the reference frame transformation (also referred to as the observer transformation). This rule of transformation should be expected, because only subscript i in FiR refers to the spatial reference frame.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

167

In the case of C, the expression is ∂xk ∂xn ∂xk ∂xn ∂ x¯ m ∂ x¯ m C¯ RS = = Qkm Qnm = Qkm Qnm ∂XR ∂XS ∂XR ∂XS ∂XR ∂XS ∂xk ∂xn ∂xk ∂xk = δkn = = CRS ∂XR ∂XS ∂XR ∂XS

(4.79)

Thus, C transforms like a scalar in the observer transformation. The left Cauchy–Green deformation tensor B transforms like ∂ x¯ i ∂ x¯ j ∂xk ∂xm B¯ ij = = Qki Qmj = Qki Qmj Bkm ∂XR ∂XR ∂XR ∂XR

(4.80)

which may be written in the matrix form as ¯ = [Q]T [B][Q] [B]

(4.81)

Thus, B transforms like a second-order tensor in the observer transformation. Consider now the observer transformation of velocity vi . Differentiating (4.69), we have D¯xi ˙ ji xj = v¯ i = Qji vj + Q Dt

(4.82)

Inverting the relation (4.69) and letting ci = 0, (4.82) becomes ˙ ji Qjk x¯ k v¯ i = Qji vj + Q

(4.83)

We see from (4.83) that vi is a ﬁrst-rank tensor, but under the observer transformation, it is not objective. If it were objective, we would have v¯ i = Qji vj for any Qij . Note that in the rigid rotation of the spatial reference frame, the spin of the frame is related to Qij through (3.184), (3.187), and (3.188), and ˙ ij Qkj = ik = ekij ωj . Therefore, given by Q v¯ = QT · v + ω × r

(4.84)

The velocity gradient is now investigated by differentiating (4.83). We obtain v¯ i,r =

∂vj ∂xs ∂ v¯ i ˙ ji Qjr = Qji Qsr vj,s + Q ˙ ji Qjr = Qji +Q ∂ x¯ r ∂xs ∂ x¯ r

(4.85)

This shows that the velocity gradient tensor is not an objective tensor either because of the presence of the second term on the right-hand side of (4.85).

© 2005 by Chapman & Hall/CRC Press

168

Continuum Mechanics and Plasticity

We show that the symmetric part of vi,j is objective, whereas the antisymmetric part of vi,j is not. To this end, we interchange i and r to obtain ∂ v¯ r ˙ jr Qji = Qjr Qsi vj,s + Q ∂ x¯ i

(4.86)

Adding (4.85) and (4.86), we ﬁnd ¯ ir = 1 D 2

∂ v¯ r ∂ v¯ i + ∂ x¯ r ∂ x¯ i

=

1 1 ˙ ˙ {Qji Qsr vj,s + Qjr Qsi vj,s } + {Q ji Qjr + Qjr Qji } 2 2 (4.87)

We note that since D ˙ ji Qjr + Q ˙ jr Qji = D (δir ) = 0 (Qji Qjr ) = Q Dt Dt

(4.88)

Equation (4.87) becomes ¯ ir = Qji Qsr Djs D

(4.89)

Therefore, Dij is an objective tensor. It is not surprising that Dij is objective, because Dij represents the rate of deformation that describes the rate of stretching of line elements, and this stretching may be measured by a ruler and is independent of the orientation of the observer. Now, let us consider the antisymmetric part of vi,j . From (4.85) and (4.86), we obtain ¯ ir = 1 W 2

∂ v¯ r ∂ v¯ i − ∂ x¯ r ∂ x¯ i

1 ˙ ˙ = Qji Qsr Wjs + (Q ji Qjr − Qjr Qji ) 2

˙ ji Qjr = Qji Qsr Wjs + Q

(4.90)

Because of the presence of the second term, the spin tensor is not objective. ˙ jr Qji = −Q ˙ ji Qjr . In The last expression has been obtained by observing that Q the case of rigid-body motion, Lij = Wij = ij , and (4.90) is reduced to ¯ ir = Qji Qsr js + ir

(4.91)

In the symbolic notation, equations (4.85), (4.89), and (4.90) are written as ˙ T · Q, L¯ = QT · L · Q + Q

(4.92a)

T

¯ = Q · D · Q, D

(4.92b)

˙T·Q ¯ = QT · W · Q + Q W

(4.92c)

It is seen that L and W depend on the spin of the rotating system, but D depends only on the orientation of the reference (spatial) frame. Note that

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

169

for two chosen coordinate systems, L transforms like a second-rank tensor if ˙ = 0. Q

4.7

Objective Rates

In the small strain mechanics, constitutive equations of the rate form have been widely used. Investigators have used the stress, stress rate, and higher-order stress rates on the one hand and the strain, strain-rate, and higher-order strainrates on the other to propose constitutive equations of the following form f (σ , σ˙ , σ¨ , . . .) = g(ε, ε˙ , ε¨ , . . .)

(4.93)

where f and g are nonlinear functions generally. When the mechanics of ﬁnite strain is of interest, we ask the question regarding the appropriate rates to use in the constitutive equations. We emphasize here that only objective tensors and objective rates can be used.

4.7.1

Some Objective Rates

Supposing that a symmetric tensor T is an objective tensor, such that T¯ = QT · T · Q

(4.94)

then, we inquire whether the rate DT/Dt is objective. If this rate is not objective, then we cannot interpret the physical signiﬁcance using it. To answer the above question, we differentiate (4.94) to obtain DT¯ D ˙ T · T · Q + QT · T˙ · Q + QT · T · Q ˙ = (QT · T · Q) = Q Dt Dt

(4.95)

The superposed “dot” denotes the material derivative. The presence of ˙ T · T · Q and QT · T · Q ˙ in (4.95) shows that T˙ is not objective. Q ˙ and Q ˙ T from (4.95), To determine an objective derivative, we eliminate Q since these terms cannot appear in a reference frame transformation. From equation (4.92a), we obtain ˙T L¯ · QT = QT · L · Q · QT + Q

or

˙ T = L¯ · QT − QT · L Q

(4.96)

By taking the transpose of (4.96), we obtain ˙ = Q · L¯ T − LT · Q Q

© 2005 by Chapman & Hall/CRC Press

(4.97)

170

Continuum Mechanics and Plasticity

By substitution, we then have from (4.95) DT¯ = (L¯ · QT − QT · L) · T · Q + QT · T˙ · Q + QT · T · (Q · L¯ T − LT · Q) Dt = L¯ · QT · T · Q − QT · L · T · Q + QT · T˙ · Q + QT · T · Q · L¯ T − QT · T · L T · Q = L¯ · T¯ − QT · L · T · Q + QT · T˙ · Q + T¯ · L¯ T − QT · T · LT · Q

(4.98)

Equation (4.98) can be rearranged into the following form DT¯ − L¯ · T¯ − T¯ · L¯ T = QT · Dt

DT − L · T − T · LT · Q Dt

(4.99)

It follows that the derivative ((DT/Dt)−L·T−T·LT ) is an objective derivative. This derivative may also be expressed in the index notation as DTij − vi,k Tkj − Tik vj,k Dt

(4.100)

Similarly, we can show that the following rates are objective rates. The Jaumann rate is given by T∇ =

DT −W·T+T·W Dt

and

T¯ ∇ = QT · T∇ · Q

(4.101)

and

T¯ ∗ = QT · T∗ · Q

(4.102)

and the convected rate is given by T∗ =

DT + LT · T + T · L Dt

The Jaumann rate deﬁned in (4.101) is based on the spin tensor W. We may use another tensor ω, which represents the rate of rotation of some physical quantity to deﬁne the same objective rate. In this case, (DT/Dt)−ω·T+T·ω is called the co-rotational rate. The physical signiﬁcance and application of these rates will be discussed later in connection with some constitutive models. Finally, we note that, if T is stress, then these are objective stress rates. EXAMPLE 4.7

Derive the convected rate.

Solution We have from (4.92a) ˙ T · Q = QT · L · Q − Q T · Q ˙ L¯ = QT · L · Q + Q

© 2005 by Chapman & Hall/CRC Press

(a)

Conservation Laws and Constitutive Equation

171

Multiplying (a) from the left by Q, we obtain ˙ Q · L¯ = L · Q − Q

˙ = L · Q − Q · L¯ or Q

(b)

Taking the transpose of (b), we have ˙ T = QT · LT − L¯ T · QT Q

(c)

Hence, after substitution of (b) and (c), (4.95) becomes DT¯ ¯ = (QT · LT − L¯ T · QT ) · T · Q + QT · T˙ · Q + QT · T · (L · Q − Q · L) Dt = QT · LT · T · Q − L¯ T · T¯ + QT · T˙ · Q + QT · T · L · Q − T¯ · L¯ = QT · (T˙ + LT · T + T · L) · Q − L¯ T · T¯ − T¯ · L¯

(d)

From (d), we write DT¯ + L¯ T · T¯ + T¯ · L¯ = QT · Dt

DT T +L ·T+T·L ·Q Dt

(e)

which shows that (DT/Dt + LT · T + T · L) is an objective rate. In the index notation, the convected rate is written as DTij + Tim vm,j + Tmj vm,i Dt EXAMPLE 4.8

(f)

Derive the Jaumann rate.

Solution From (4.92), we have ¯ = QT · W · Q + Q ˙ T · Q = QT · W · Q − Q T · Q ˙ W

(a)

Multiplying (a) by Q from the left, we have ¯ =W·Q−Q ˙ Q·W

˙ =W·Q−Q·W ¯ or Q

(b)

Taking the transpose of (b), we obtain ˙ T = QT · WT − W ¯ T · QT Q

© 2005 by Chapman & Hall/CRC Press

(c)

172

Continuum Mechanics and Plasticity

Substituting (b) and (c) into (4.95), we ﬁnd DT¯ ¯ T · QT ) · T · Q + QT · T˙ · Q + QT · T · (W · Q − Q · W) ¯ = (QT · WT − W Dt ¯ T · T¯ + QT · T˙ · Q + QT · T · W · Q − T¯ · W ¯ = QT · W T · T · Q − W ¯ T · T¯ − T¯ · W ¯ = QT · (T˙ + WT · T + T · W) · Q − W

(d)

From (d) we conclude that DT¯ ¯ T · T¯ + T¯ · W ¯ = QT · +W Dt

DT + WT · T + T · W · Q Dt

(e)

DT −W·T+T·W ·Q Dt

(f)

But WT = −W, (e) then becomes DT¯ ¯ · T¯ + T¯ · W ¯ = QT · −W Dt

Therefore, T∇ =

DT −W·T+T·W Dt

(g)

is an objective rate.

4.7.2

Physical Meaning of the Jaumann Stress Rate

Let a body spin with an angular velocity w with reference frame at time t denoted by xi . Let x¯ i be another reference frame which is attached to the body and spins with it. Let x¯ i coincide with xi at time t, when the stress at a generic point P in the body is σ¯ ij (t) = σij (t). At time t + dt, the stress at particle P is σ¯ ij (t + dt) referred to the rotating axes x¯ i . Then, according to Jaumann, the stress rate may be deﬁned as 1 [σ¯ ij (t + t) − σ¯ ij (t)] t→0 t

σij∇ = lim

(4.103)

The relation Qij between the two reference frames may be found by considering the spin of the reference frame (see Figure 4.7) which rotates base vectors ei into e¯ i . From (1.22), the relation is e¯ i = Qji ej

© 2005 by Chapman & Hall/CRC Press

(4.104)

Conservation Laws and Constitutive Equation

173

–

ei dt

dei

ei FIGURE 4.7 Spin of the reference frame.

The angle of rotation is ω dt, where ω is the angular velocity. Using n to denote the unit normal to the plane formed by ei and e¯ i , the angular velocity vector is w = ωn = ωni ei = wi ei

(4.105)

Therefore, wi = ωni . Referring to Figure 4.7, we write e¯ i = ei + dei = ei + w dt × ei

(4.106)

Using (4.104), (4.106) becomes Qji ej = ei + ωnj dtej × ei = ei + ωnk dt eijk ej

(4.107)

The components of (4.107) are Qji = δij + ωnk dteijk

(4.108)

Qij = δij − ωnk dteijk

(4.109)

which may be rewritten as

Equation (4.109) describes the rotation of the reference frame. This equation may be compared with (1.118) and the same result can be obtained from (1.118) by setting cos α = 1, sin α = α, α = ω dt, and wk = ωnk . The stress tensor at P at time t + dt referred to the reference frame xi is

σij (t + dt) = σij (t) +

© 2005 by Chapman & Hall/CRC Press

Dσij dt Dt

(4.110)

174

Continuum Mechanics and Plasticity

The stresses σ¯ ij (t+dt) and σij (t+dt), referring to x¯ i and xi systems, respectively, are related by σ¯ ij = Qpi Qqj σpq , so that by use of (4.109), we write σ¯ ij (t + dt) = Qpi Qqj σpq (t + dt)

Dσpq = (δpi − epim wm dt)(δqj − eqjn wn dt) σpq (t) + dt Dt Dσij = σij (t) + − epim wm σpj − eqjn wn σiq dt + O(dt2 ) Dt (4.111)

Hence, by neglecting the higher order terms in dt and using (4.103), we obtain σij∇ =

Dσij − epim wm σpj − eqjn wn σiq Dt

(4.112)

Noting that Wjk = −eijk wi

and

−Wjq = Wqj

(4.113)

we then have σij∇ =

D σij − Wip σpj + σiq Wqj Dt

(4.114)

This is the Jaumann stress rate and is the same as the expression in (4.101).

4.8

Finite Elasticity

We study the topic of elasticity in the remaining part of this chapter. Elasticity investigates the speciﬁc material behavior which is reversible, that is, if a material is elastic, then upon the removal of loading, the material will recover its original state. Elastic material is an ideal material and it is a good approximation for most materials in the small strain range. In the ﬁnite strain range, rubber is known to exhibit an elastic behavior to a good approximation. There are several approaches to formulating the constitutive equation for an elastic material. The Cauchy elasticity is discussed ﬁrst and then the hyperelasticity. Emphasis is given to hyperelasticity and provide several examples in the application. Finally, in the last section of this chapter, hypo-elasticity is discussed, which, strictly speaking, is not elasticity.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation 4.8.1

175

The Cauchy Elasticity

In the investigation of a constitutive equation, we consider the stress and deformation of an inﬁnitesimal material element. If the material is elastic, then the stress σ is, by deﬁnition, a function of the current deformation written as σ = g(F)

(4.115)

where g is a tensor-valued function of F and is in general a nonlinear function. We use the deformation gradient F to denote deformation for the purpose of generality, and we show next by use of objectivity that the deformation cannot be represented by F. Under observer transformation of (4.69), an arbitrary QT , (4.115) is written in the barred frame as ¯ σ¯ = g(F)

(4.116)

which by use of (4.71) and (4.72) is QT · σ · Q = g(QT · F)

(4.117)

QT · g(F) · Q = g(QT · F)

(4.118)

or

for an arbitrary orthogonal Q. Equation (4.118) gives the restriction on the form of g in (4.115). In particular, if we choose Q = R and, by applying F = R · U from the polar decomposition theorem, we obtain QT · F = RT · F = RT · R · U = U

(4.119)

Note that the observer transformation is valid for any Q, but if we make a special choice of it, we can observe useful information from this orientation of the observer. The information is still there, but it cannot be visualized from another orientation Q. Making use of (4.119), (4.118) becomes RT · g(F) · R = g(U)

(4.120)

Combining (4.115) and (4.120), we obtain σ = R · g(U) · RT

(4.121)

We see from (4.121) that σ depends on a nonlinear function of U and depends on R explicitly. But, since U is related to C from (3.40) and C is related to E from (3.100), equivalent forms of (4.121) are σ = R · f(C) · RT

© 2005 by Chapman & Hall/CRC Press

(4.122)

176

Continuum Mechanics and Plasticity

and σ = R · h(E) · RT

(4.123)

where f is a tensor-valued function of C and h is a tensor-valued function of E. One of (4.121), (4.122), or (4.123) may be used as the constitutive equation for anisotropic elastic materials. For a given deformation, R, U, C, and E can be determined. If explicit functions g, f, or h are known, then by use of one of the above constitutive equations the stress σ may be determined. In the case that the material is isotropic, (4.122) may be rewritten as σˆ ≡ RT · σ · R = f(C)

(4.124)

Following a representation theorem of Rivlin and Ericksen [1] for an isotropic tensor function of a tensor, (4.124) is written as σˆ = ϕ0 1 + ϕ1 C + ϕ2 C2

(4.125)

where ϕ0 , ϕ1 , and ϕ2 are scalar invariant functions of the three principal invariants of C. Equation (4.125) can also be derived by expressing the function f in (4.124) as a polynomial of C and applying the Cayley–Hamilton theorem (Section 2.15) successively. From (2.104), we write C3 = I1 C2 − I2 C + I3 I

(4.126)

where I1 , I2 , and I3 are principal invariants of C. By successive applications of (4.126), (4.124) reduces to (4.125). From (4.125), we have σ = R · σˆ · RT = R · (ϕ0 1 + ϕ1 C + ϕ2 C2 ) · RT = ϕ0 R · RT + ϕ1 R · C · RT + ϕ2 R · C · CT · RT

(4.127)

The last term of (4.127), using (3.37), is R · C · CT · RT = R · C · (RT · R) · CT · RT = (R · C · RT ) · (R · C · RT )T = B · BT (4.128) Substituting (3.37) and (4.128) into (4.127), we obtain σ = ϕ0 1 + ϕ1 B + ϕ2 B2

(4.129)

where ϕk = ϕk (I1 , I2 , I3 ) and we note that the principal invariants of C and B are the same. By use of the Cayley–Hamilton theorem, (4.129) may be written in a slightly different form. From (2.104), we write B3 − I1 B2 + I2 B − I3 1 = 0

© 2005 by Chapman & Hall/CRC Press

(4.130)

Conservation Laws and Constitutive Equation

177

Multiplying (4.130) by B−1 , we get B2 = I1 B − I2 1 + I3 B−1

(4.131)

Finally, we substitute (4.131) into (4.129) to obtain σ = α0 1 + α1 B + α−1 B−1

(4.132)

where α0 = ϕ0 − ϕ2 I2 ,

α1 = ϕ1 + ϕ2 I1 ,

α−1 = ϕ2 I3

(4.133)

Either (4.129) or (4.132) can be used as the constitutive equation for an isotropic elastic material. 4.8.2

Hyperelasticity

A material is called hyperelastic or Green-elastic if there exists an elastic potential function, widely known as the strain-energy density function W , which is a scalar function of one of the strain or deformation tensors. Hyperelasticity uses the conservation of energy principle, leaving out the thermal effect. We postulate that the elastic material is capable of storing strain-energy and write Rate of work done on body R

Rate of change of strain-energy in R

=

(4.134)

It may be shown that the strain-energy density is equal to the Helmholz free energy for isothermal process and is equal to the internal energy for isentropic process. This is further discussed in a later chapter. But, we mention for now that the free energy is the portion of internal energy available for doing work at constant temperature. If the strain-energy density W is deﬁned per unit undeformed volume, then Total strain-energy =

W dV0 =

W

dV0 dV = dV

ρ W dV ρ0

(4.135)

The rate of change of the strain-energy is then D Dt

ρ W dV = ρ0

ρ DW dV ρ0 Dt

(4.136)

and the rate of work done is (n) ti vi dS = σki nk vi dS = (σki vi ),k dV = (σki,k vi + σki vi,k ) dV S

S

V

V

(4.137)

© 2005 by Chapman & Hall/CRC Press

178

Continuum Mechanics and Plasticity

But the term V (σki,k vi )dV in (4.137) cancels out with the kinetic energy term and the body force term by use of the equation of motion as discussed in Section 4.3.3. Therefore, the rate of work done that affects the rate of change of strain-energy is V

σki vi,k dV

(4.138)

Substituting (4.136) and (4.138) into (4.134), this balance of energy in the local form, is given by ρ DW ∂vi ∂XR = σji vi,j = σji ρ0 Dt ∂XR ∂xj

(4.139)

or by use of (4.42) ρ0 ∂XR ∂vi DW (0) ∂vi (0) ∂ = TRi = TRi = σji Dt ρ ∂xj ∂XR ∂XR ∂XR ∂xi (0) D (0) DFiR = TRi = TRi Dt ∂XR Dt

Dxi Dt

(4.140)

(0)

where TRi is the 1st P–K stress. In the case of elastic material, the stress is a function of current deformation. If the deformation is expressed by the deformation gradient FiR , the strainenergy density W is a function of FiR . Thus, DW (FiR ) ∂W DFiR = Dt ∂FiR Dt

(4.141)

By the substitution of (4.141) into (4.140), we then obtain

∂W (0) − TRi ∂FiR

DFiR =0 Dt

(4.142) (0)

Since this equation should hold for all DFiR /Dt and since W and TRi are functions of FiR , but independent of DFiR /Dt, the left-hand side of the above equation must vanish for all arbitrary value of DFiR /Dt. It follows that (0)

TRi =

∂W ∂FiR

(4.143)

or, by use of (4.42), σij =

© 2005 by Chapman & Hall/CRC Press

∂W ρ ∂xi ∂W (F) ρ = FiR ρ0 ∂XR ∂FjR ρ0 ∂FjR

(4.144)

Conservation Laws and Constitutive Equation

179

This is the most general constitutive equation of an elastic material undergoing ﬁnite deformation if we make use of the strain-energy density function. In the last step, the symmetric property of σij is invoked. We now consider the effect of objectivity on the form of strain-energy function W . By applying objectivity, we have in the barred reference frame σij =

¯ ¯ ∂FrS ∂W ρ ¯ ∂W ρ FiR = F¯ iR ρ0 ρ0 ∂FrS ∂ F¯ jR ∂ F¯ jR

(4.145)

But, from (4.78), F¯ iR = Qki FkR ,

FrS = Qrm F¯ mS ,

∂FrS = Qrm δmj δSR = Qrj δSR ∂ F¯ jR

(4.146)

Hence, after substitution, (4.145) becomes σ¯ ij =

¯ ¯ ∂W ρ ∂W ρ Qki FkR Qrj δSR = Qki Qrj FkR ρ0 ∂FrS ρ0 ∂FrR

(4.147)

Therefore, by comparing (4.147) with (4.144), we conclude that σ¯ ij = Qki Qrj σkr

or

σ¯ = QT · σ · Q

¯ (F) ¯ if W (F) = W

(4.148)

which states that objectivity of the stress tensor is satisﬁed if the strain-energy density W is form-invariant with rotation of the spatial reference frame. Hence, ¯ (F) ¯ = W (F) ¯ = W (F) W

(4.149)

The last equality is equivalent to the condition that W (QT · F) = W (F)

for any orthogonal Q

(4.150)

In particular, if we choose Q = R and, by applying F = R · U from the polar decomposition theorem, we obtain QT · F = R T · F = R T · R · U = U

(4.119)

as in the discussion of the Cauchy elasticity. Therefore, by substituting (4.119) into (4.150), we obtain W (F) = W (U)

© 2005 by Chapman & Hall/CRC Press

(4.151)

180

Continuum Mechanics and Plasticity

which means that W depends on F only through its dependence on U. But, since U is related to C by (3.40), the strain-energy density may also be expressed in terms of C as √ ˜ (C) = W (C) W (U) = W ( C) = W

(4.152)

The tilde in the last expression has been dropped for simplicity. We may do this, since the function is as yet unspeciﬁed. We have thus shown from the application of objectivity that the strain-energy density function is a function of the right Cauchy–Green deformation tensor C. Using this property, we now have ∂W ∂W ∂CST ∂W ∂((∂xi /∂XS )(∂xi /∂XT )) = = ∂FjR ∂CST ∂FjR ∂CST ∂(∂xj /∂XR ) ∂W ∂xi ∂xi = δij δSR + δij δTR ∂CST ∂XT ∂XS =

∂W ∂xj ∂W ∂xj ∂W ∂xj + =2 ∂CRT ∂XT ∂CSR ∂XS ∂CSR ∂XS

(4.153)

Note that the last equality is obtained by observing the symmetric property of CRS . Therefore, the stress of equation (4.144) can be written as σij = 2

ρ ∂xi ∂xj ∂W ρ0 ∂XR ∂XS ∂CRS

(4.154)

In terms of the 2nd P–K stress tensor, the constitutive equation for hyperelastic material is given from (4.48) and (4.154) by

RS = Jσjk =2

∂xj ∂xk ∂W ∂XR ∂XS ∂XR ∂XS =2 ∂xj ∂xk ∂XP ∂XQ ∂CPQ ∂xj ∂xk

∂W ∂W δPR δQS = 2 ∂CPQ ∂CRS

(4.155)

Hence,

RS = 2

∂W (C) ∂W (E) = ∂CRS ∂ERS

(4.156)

where ERS is the Lagrangian strain tensor deﬁned by (3.100). It is seen that by use of the 2nd P–K stress, the stress is the partial derivative of the strainenergy density function with respect to a deformation tensor. The constitutive equation is thus greatly simpliﬁed. We note that this equation applies to fully anisotropic elastic materials.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation 4.8.3

181

Isotropic Hyperelastic Materials

A material is said to be isotropic, if its constitutive equation remains forminvariant with rotation of the material coordinate system XR . This statement is similar to that of material objectivity. The difference is that we rotate the material coordinate system here. The isotropic statement imposes a constraint on the constitutive equations (4.154) and (4.156), and, since in hyperelasticity the stress is expressed in terms of the strain-energy density function, the constraint of isotropy is imposed on the strain-energy density W(C). Therefore, we state that an elastic material is isotropic if its strain-energy density function is form-invariant with rotation of the material coordinate system. Anecessary and sufﬁcient condition that W (C) be form-invariant with rotation of the material coordinate system is that W is a function only of the invariants of CRS , and not a function of the components of CRS .

THEOREM

Proof From the spectral representation (2.95) of a symmetric second-rank tensor by its eigenvalues and eigenvectors, we write CRS =

(Q)

(Q)

CQ N R N S

(1)

(1)

(2)

(2)

(3)

(3)

= C1 N R N S + C 2 N R N S + C 3 N R N S

(4.157)

Q

Then, the strain-energy density function is given by (1)

(2)

(3)

W = W (C1 , C2 , C3 ; NR , NR , NR

(4.158) (Q)

where the eigenvalues CQ remain invariant on the rotation of XR ; and NR are the eigenvectors. We now make use of a theorem on invariants (see Green and Adkins [2]) which states that: a scalar-valued function φ(α(1) , α(2) , . . . , α(m) ) of m vectors α(1) , α(2) , . . . , α(m) is invariant under all proper orthogonal transformations if and only if it can be expressed as a function of all possible inner products α(r) · α(s) (r, s = 1, 2, . . . , m) and the determinant |α(r) |, that is, φ = φ(α(r) · α(s) , |α(r) |)

(4.159)

In the case of (4.158), the eigenvectors are orthogonal so that (P)

(Q)

N R NR

= δPQ

and

(P)

|NR | = 1

(4.160)

Therefore, the strain-energy function is W = W (C1 , C2 , C3 )

© 2005 by Chapman & Hall/CRC Press

(4.161)

182

Continuum Mechanics and Plasticity

In the above expression, the indices 1, 2, and 3 are arbitrarily chosen depending on the designation of the coordinate axes. Since W must be a symmetric function of C1 , C2 , and C3 , it must be form-invariant with permutation of the indices, that is, W (C1 , C2 , C3 ) = W (C1 + C2 + C3 , C1 C2 + C2 C3 + C3 C1 , C1 C2 C3 )

(4.162)

or W = W (I1 , I2 , I3 )

(4.163)

where I1 , I2 , and I3 are the three principal invariants of CRS deﬁned in Section 3.6.4 and this concludes the proof of the theorem. To obtain the constitutive equation for isotropic hyperelastic material, we consider ∂W ∂I1 ∂W ∂I2 ∂W ∂I3 ∂W = + + ∂CRS ∂I1 ∂CRS ∂I2 ∂CRS ∂I3 ∂CRS

(4.164)

where ∂I1 = δRS, ∂CRS

∂I2 = I1 δRS − CRS, ∂CRS

∂I3 −1 = cofactor(CRS ) = I3 CRS ∂CRS (4.165)

The expressions for the three invariants are given in Sections 2.12 and 3.6.4. In particular, we mention here that I2 = 12 (I12 − CRS CRS )

(4.166)

By substitution, we then obtain from (4.156)

RS = 2

∂W ∂W ∂I1 ∂W ∂I2 ∂W ∂I3 =2 + + ∂CRS ∂I1 ∂CRS ∂I2 ∂CRS ∂I3 ∂CRS

(4.167)

or

RS = 2

∂W −1 ∂W ∂W δRS + (I1 δRS − CRS ) + I3 C ∂I1 ∂I2 ∂I3 RS

(4.168)

To express the above equation in terms of the Cauchy stress, we obtain from (4.50) σij =

© 2005 by Chapman & Hall/CRC Press

ρ ∂xi ∂xj

RS ρ0 ∂XR ∂XS

(4.169)

Conservation Laws and Constitutive Equation

183

Using (4.168), each term in (4.169) needs to be multiplied by a factor and these terms are ∂xi ∂xj ∂xi ∂xj δRS = = Bij = left Cauchy–Green tensor ∂XR ∂XS ∂XR ∂XR ∂xi ∂xj ∂xi ∂xj CRS = ∂XR ∂XS ∂XR ∂XS

∂xk ∂xk ∂XR ∂XS

=

∂xi ∂xk ∂XR ∂XR

∂xk ∂xj ∂XS ∂XS

(4.170) = Bik Bkj (4.171)

∂xi ∂xj ∂XR ∂XS ∂xi ∂xj −1 C = ∂XR ∂XS RS ∂XR ∂XS ∂xk ∂xk ∂xj ∂XS ∂xi ∂XR = = δik δjk = δij ∂XR ∂xk ∂XS ∂xk

(4.172)

By substituting these expressions into (4.168) and (4.169), we obtain 2 σij = √ I3

∂W ∂W ∂W Bij + (I1 Bij − Bik Bkj ) + I3 δij ∂I1 ∂I2 ∂I3

(4.173)

or 2 σij = √ I3

∂W ∂W + I1 ∂I1 ∂I2

∂W ∂W Bij − Bik Bkj + I3 δij ∂I2 ∂I3

ρ0 2 with I3 = ρ (4.174)

Equation (4.174) is the constitutive equation for isotropic hyperelasticity and we observe that the scalar coefﬁcients of (4.174) are derived from a single scalar function W (I1 , I2 , I3 ). Equation (4.174) has the same form as the constitutive equation (4.129) of Cauchy elasticity. But, in the case of Cauchy elasticity, there are three scalar functions ϕk (I1 , I2 , I3 ) which need to be determined from experiments. We now discuss the constraints due to incompressibility. Under moderate stress 10,000 psi (68.9 MPa), the assumption of incompressibility is valid for rubber. When the material is incompressible, we can write I3 =

ρ0 ρ

2

=1

(4.175)

In this case ∂W /∂I3 |I3 =1 is indeterminate and is no longer a material property. Incompressibility is a kinematic constraint expressed by vi,i = Dii = 0. The mechanical effect of such a constraint is to give rise to an arbitrary hydrostatic pressure −p1 which does no work. From the energy equation (4.34),

© 2005 by Chapman & Hall/CRC Press

184

Continuum Mechanics and Plasticity

the term σki vi,k = σki Dik is not affected by superimposed hydrostatic pressure, that is, (σki − pδki )Dik = σki Dik − pδki Dik = σki Dik − pDii = σki Dik

(4.176)

Incompressible materials are capable only of isochoric deformations. The arbitrary hydrostatic pressure is not given by a constitutive equation but is determined by the equations of motion (or equilibrium) and boundary conditions. In this case, the strain-energy density function is written as W (I1 , I2 ) and from (4.173) the hyperelastic constitutive equation for incompressible material is written as σij = 2{W1 Bij + W2 (I1 Bij − Bik Bkj ) − pδij }

(4.177)

where Wi = ∂W /∂Ii . By use of the Cayley–Hamilton theorem (4.177) may also be written as σij = −pδij + 2W1 Bij − 2W2 B−1 ij

(4.178)

EXAMPLE 4.9 The hydrostatic pressure is expressed in the form of Cauchy stress by σij = −pδij . Find corresponding expressions using the 1st and 2nd P–K stresses and discuss the physical meanings of these expressions, if any. Consider cases where the deformation gradient F has or does not have a diagonal form.

Solution From (4.42) and (4.48), we have ∂XR ∂XR = −Jp ∂xj ∂xi

(a)

∂XR ∂XS ∂XR ∂XS −1 = −Jp = −JpCRS ∂xj ∂xk ∂xk ∂xk

(b)

(0)

TRi = −Jpδji

RS = −Jpδjk

If F has a diagonal form such as

λ1 [F] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 λ2 0

0 0 λ3

1 λ1 −1 [F ] = 0 0

0 1 λ2 0

0

0 1 λ3

(c)

Conservation Laws and Constitutive Equation

185

then (a) and (b) become

(0)

TRi

1 λ1 = −Jp 0 0

0 1 λ2 0

0

0 1 λ3

RS

1 λ2 1 = −Jp 0 0

0

0

1 λ22 0

0 1

(d)

λ23

There are only normal components in both stress tensors and the sum of the diagonal terms for both cases are

tr T

(0)

1 1 1 = −Jp + + λ1 λ2 λ3

tr = −Jp

1 λ21

+

1 λ22

+

1 λ23

(e)

We see from (e) that both tr T(0) and tr are multiples of the hydrostatic stress p, but affected by the stretching or contraction of the material element through λi . (0) If F does not have the diagonal form, then both TRi and RS do not have the diagonal form. In other words, even though we can still ﬁnd tr T(0) and tr and both are multiples of the hydrostatic stress p, shear stresses arise in (0) both TRi and RS so that it is fair to say that the 1st and 2nd P–K stresses are hydrostatic pressure sensitive, while the Cauchy stress is not. The shear components of the Cauchy stress are not affected by the superimposed hydrostatic pressure.

4.8.4

Applications of Isotropic Hyperelasticity

This section discusses some simple applications of the constitutive equation for isotropic hyperelasticity. If the strain-energy function W is known for an incompressible material, then the stress is determined by (4.177) or (4.178) up to a hydrostatic pressure, which is in turn determined from the boundary condition. The complexity of the governing equations usually calls for numerical means to solve them. However, some simple problems may be solved by the inverse method. In this method, we ﬁrst assume a suitable form for the deformation and then use the constitutive equations to ﬁnd the associated stresses and consider the restrictions imposed by the equations of equilibrium. Finally, we determine the surface tractions necessary to maintain the deformation. These simple problems serve to illustrate the method of solution in ﬁnite elasticity, and some of these problems have added importance in that they may be experimentally investigated. They are then used to determine the form of the strain-energy function of a given elastic material. The following

© 2005 by Chapman & Hall/CRC Press

186

Continuum Mechanics and Plasticity

two forms of the strain-energy function are well known. They are W = C(I1 − 3)

(4.179)

W = C1 (I1 − 3) + C2 (I2 − 3)

(4.180)

and

in which C, C1 , and C2 are constants. Form (4.179) is known as the Neo-Hookean form which was derived from kinetic theory of rubber by Treloar. Form (4.180) is known as the Mooney form or the Mooney–Rivlin form. Following Rivlin [3], the strain-energy function W = W (I1 , I2 , I3 ) of an isotropic material, which is normally expressed in a polynomial of I1 , I2 , and I3 , may be equally expressed as a polynomial function of (I1 − 3), (I2 − 3), and (I3 − 1). Thus,

W=

Aαβγ (I1 − 3)α (I2 − 3)β (I3 − 1)γ

(4.181)

α,β,γ

where Aαβγ are constants. When the material is undeformed, C11 = C22 = C33 = 1, and I1 − 3 = 0, I2 − 3 = 0, I3 − 1 = 0. Following this approach, the strain-energy function for incompressible material is given by W=

Aαβ (I1 − 3)α (I2 − 3)β

(4.182)

α,β

4.8.4.1 Uniaxial extension In the case of uniform extensions, the deformation is given by (3.18). Using (3.18), we ﬁnd

λ21

[B] = 0

0

0

0

λ22

0 ,

0

λ23

λ41

[B2 ] = 0

0

0

0

λ42

0

0

λ43

(4.183)

Substituting (4.183) into (4.177), we obtain σ11 = 2{W1 λ21 + W2 (I1 λ21 − λ41 ) − p}

(4.184a)

σ22 = 2{W1 λ22 + W2 (I1 λ22 − λ42 ) − p}

(4.184b)

σ33 = 2{W1 λ23 + W2 (I1 λ23 − λ43 ) − p}

(4.184c)

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

187

For uniaxial test, σ22 = σ33 = 0. Using these conditions and subtracting (4.184b) from (4.184a), we obtain σ11 = 2{W1 (λ21 − λ22 ) + W2 [I1 (λ21 − λ22 ) − (λ41 − λ42 )]}

(4.185)

which reduces to σ11 = 2(λ21 − λ22 ){W1 + W2 (I1 − λ21 − λ22 )}

(4.186)

σ11 = 2(λ21 − λ22 ){W1 + λ23 W2 }

(4.187)

or

The expression I1 = λ21 + λ22 + λ23 was used to arrive at this equation. In addition, by subtracting (4.184c) from (4.184b), we obtain 0 = 2(λ22 − λ23 ){W1 − λ21 W2 }

(4.188)

This quantity must vanish for all λ1 and, therefore, λ2 = λ3 . If the material is incompressible, then det F = 1, so that λ1 λ22 = 1

with λ2 = λ3

(4.189)

Hence, by substituting (4.189) into (4.187), we obtain 1 + W = 2 W 1 2 λ1 λ21 − (1/λ1 ) σ11

(4.190)

In the experiments of uniaxial tension and compression, σ11 and λ1 may be measured and the left-hand side of (4.190) may be calculated. The details of the experiments are reported in Rivlin and Saunders [4] from vulcanized rubber test-pieces. The experimental results show that when σ11 /(λ21 − λ−1 1 ) is plotted against 1/λ1 , the material response for the case of 1/λ1 < 1 (tension) is quite different from that for the case of 1/λ1 > 1 (compression). The experimental data in the tension zone and in the compression zone can be best ﬁtted by the Mooney form (4.180) and the Neo-Hookean form (4.179), respectively. Figure 4.8 shows a schematic plot of the two models each applied in the recommended zone. 4.8.4.2

Simple shear

The simple shear deformation has been previously discussed in Section 3.4.1.2 and Example 3.3. The transformation equations for this deformation are x1 = X1 + kX2 ,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(4.191)

188

Continuum Mechanics and Plasticity

Tension

– 2 1

11

–1 1

Compression Neo-Hookean form

ey on Mo m for

1/1

1.0 FIGURE 4.8 Uniaxial tension and compression.

where k is a nonzero constant, and, based on (4.191), we ﬁnd

1 + k2 [B] = k 0

k 0 1 0 0 1

1 [B−1 ] = −k 0

−k 1 + k2 0

0 0 1

(4.192)

with I1 = 3 + k 2 ,

I2 = 3 + k 2

and

I3 = 1

(4.193)

Thus, there is no change in volume during simple shearing. Using the hyperelastic constitutive equation (4.178), we ﬁnd σ11 = −p + 2(1 + k 2 )W1 − 2W2

(4.194a)

σ22 = −p + 2W1 − 2(1 + k 2 )W2

(4.194b)

σ33 = −p + 2W1 − 2W2

(4.194c)

σ12 = kµ(k 2 )

σ23 = σ31 = 0

(4.194d)

in which the hydrostatic pressure p is to be determined by the prescribed boundary conditions and µ(k 2 ) = 2(W1 + W2 )

(4.194e)

where µ(k 2 ) is usually referred to as the generalized shear modulus. We note that k is the shear strain, and when we reverse the direction of shear, we change the sign of the shear stress. This is satisﬁed only when µ(k 2 ) > 0. In the case of small deformations, it is known that the simple shear deformation can be maintained by applying only shear stresses without normal

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

189

stresses on the faces of the specimen. In a ﬁnite deformation, we inquire whether this is still true, for shear strain k = 0. By setting σ11 = σ22 = σ33 = 0, we obtain from (4.194) that −p + 2(1 + k 2 )W1 − 2W2 = 0 −p + 2W1 − 2(1 + k 2 )W2 = 0

(4.195)

−p + 2W1 − 2W2 = 0 Solving the set of equations in (4.195) for a nontrivial solution for −p, 2W1 , and −2W2 , the determinant of the coefﬁcient matrix has to be zero. Thus, 1 1 + k 2 1 1 1 1

1 1 + k 2 = k 4 = 0 1

(4.196)

We obtain from (4.196) that k = 0, which corresponds to no shear deformation and is in contradiction with the assumption that k = 0. On the other hand, the trivial solution of p = W1 = W2 = 0, from (4.194a–e), leads to µ(k 2 ) = 0 and σ12 = σ11 = σ22 = σ33 = 0, that is, the shear strain k = 0 gives rise to no stresses, in contradiction with experimental observations. We therefore conclude that the simple shear deformation cannot be maintained by applying only shear stresses on the faces of the specimen. Generally, normal stresses must also be applied. From (4.194), the mean stress is 1 3 σkk

= (−p + 2W1 − 2W2 ) + 23 k 2 (W1 − W2 )

(4.197)

When k, −p, W1 , and W2 are all nonzero, then (4.197) gives rise to a nonzero mean stress. If normal stresses are not applied, then the material element will either expand or contract in volume according to the sign of the mean stress. However, this deformation is not a simple shear deformation. From (4.194a–e), we may also obtain σ11 − σ22 = kσ12

(4.198)

This relation does not depend on the form of the strain-energy function. An implication of this equation is that during shearing, the normal stresses σ11 and σ22 cannot be equal. The existence of these unequal normal stresses is called the Poynting effect. This effect was ﬁrst investigated by Poynting [5] who performed a series of torsion experiments on metal wires and observed the lengthening of wires when no axial force was applied. This effect is also known as the axial effect and is discussed later related to plastic deformation. In order to maintain the simple shear deformation, normal stress σ N and shear stress σ S must be applied on the inclined faces of the deformed

© 2005 by Chapman & Hall/CRC Press

190

Continuum Mechanics and Plasticity 2

22 12

D

C

22 S

12 s

11

n

A

N 1

B

FIGURE 4.9 Simple shear.

specimen. These stresses are now calculated. Referring to Figure 4.9, the outward normal n to the inclined surface BC has components [n] = [cos γ , − sin γ , 0]

(4.199)

where the angle γ is deﬁned by k = tan γ , with sin γ = k/ 1 + k 2 and cos γ = 1/ 1 + k 2 . The unit tangential vector s has components [s] = [sin γ , cos γ , 0]

(4.200)

The normal and shear components are then

σ N = σij nj ni = [cos γ

− sin γ

σ11 0] σ12 0

σ12 σ22 0

0 cos γ 0 − sin γ σ33 0

= σ11 cos2 γ + σ22 sin2 γ − σ12 sin 2γ σ S = σij nj si =

(4.201)

(σ11 − σ22 ) sin 2γ + σ12 cos 2γ 2

(4.202)

Since sin 2γ = 2k/(1 + k 2 ), cos 2γ = (1 − k 2 )/(1 + k 2 ), and σ11 − σ22 = kσ12 , it is easily shown that σ N = σ22 − kσ S

and

σS =

σ12 1 + k2

(4.203)

We now see that σ S < σ12 and σ N < σ22 . This assures that if σ22 is in compression and is negative, so is σ N in compression.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

191

F

F

2

1 3 FIGURE 4.10 Biaxial compression of a cubic block.

EXAMPLE 4.10

Find the state of stress in the biaxial compression of a cubic

block. Solution This test is sometimes referred to as the conﬁned compression test. Referring to Figure 4.10, the block is conﬁned in the 2-direction, while a compressive force F is applied in the 1-direction. The 3-direction is free. The deformation is governed by x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

(a)

and we ﬁnd from (a)

λ1 [F] = 0 0

0 λ2 0

0 0 , λ3

λ21

0

0

[B] = 0

λ22

0 ,

0

0

λ23

λ41

0

0

[B2 ] = 0

λ42

0

0

0

λ43 (b)

with |F| = λ1 λ2 λ3 = λ1 λ3 = 1. We used λ2 = 1, since the block cannot deform along the 2-direction. The stresses are found by putting (b) into (4.177), which leads to (4.184a–c). Because the 3-direction is free, we write σ33 = 0. Using this constraint, (4.184c) becomes p = W1 λ23 + W2 (I1 λ31 − λ43 )

(c)

Substituting (c) into (4.184a), we then obtain σ11 = 2{W1 λ21 + W2 (I1 λ21 − λ41 ) − W1 λ23 − W2 (I1 λ23 − λ43 )}

© 2005 by Chapman & Hall/CRC Press

(d)

192

Continuum Mechanics and Plasticity

The ﬁrst invariant of B is I1 = λ21 + λ22 + λ23 = λ21 + 1 +

1

(e)

λ21

Applying (e), (d) may be further reduced to λ21

σ11 = 2

−

1

{W1 + W2 }

λ21

(f)

Similarly, we obtain the following equation from (4.184b) σ22 = 2 1 −

1

{W1 + W2 λ21 }

λ21

(g)

For the Neo-Hookean form given by (4.179), W1 = C and W2 = 0. The stresses are found from (f) and (g) as σ11 = 2

λ21

−

1 λ21

σ22 = 2 1 −

C,

1

λ21

C = constant

C,

(h)

From (h), we ﬁnd the following stress ratio which indicates a conﬁned stress in the 2-direction ξ=

1 σ22 = σ11 1 + λ21

(i)

Equation (i) is plotted against λ1 in Figure 4.11. We note that ξ = 1.0 when λ1 = 0; ξ = 0.5 when λ1 = 1; and ξ = 0 when λ1 → ∞. For the Mooney form given by (4.180), W1 = C1 and W2 = C2 . The stresses are found from (f) and (g) as σ11 = 2

λ21

−

1 λ21

{C1 + C2 },

σ22 = 2 1 −

1 λ21

C1 , C2 = constants

C1 + C2 λ21 , (j)

From (j), we ﬁnd the following stress ratio ξ=

C1 + C2 λ21 σ22 = σ11 (1 + λ21 )(C1 + C2 )

(k)

We see from (k) that ξ = C1 /(C1 + C2 ) when λ1 = 0; ξ = 0.5 when λ1 = 1; and ξ = C2 /(C1 + C2 ) when λ1 → ∞. The exact shape of the curve depends on the values of C1 and C2 . In a special case when C1 = C2 , we obtain ξ = 0.5 for

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

Neo-Hookean Mooney

1

0.5

193

C1 C1 + C2 C2 C 1 + C2

0

0.5

1

Compression

1.5

2

1

Tension

FIGURE 4.11 The ξ ratio plotted against λ1 .

all λ1 . According to Rivlin and Saunders [4], W1 > W2 for vulcanized natural rubber, and, therefore, C1 > C2 . Equation (k) is plotted in Figure 4.11 for the case of C1 = 2.5C2 (C1 > C2 ). We note that the conﬁning stress σ22 is always smaller than σ11 for both models. They are equal only in the Neo-Hookean model when λ1 = 0, which is a limiting case and cannot realistically happen.

4.9 4.9.1

Inﬁnitesimal Theory of Elasticity Constitutive Equation

We showed in Section 3.9.1 that, in the case of small displacement gradient, it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi . Thus, the inﬁnitesimal strain tensor εij = 12 (ui,j + uj,i )

(4.204)

can and will be used. In this case, both Lagrangian strain E and Enlerian strain e reduce to ε. There are no distinctions among different stress measures and σij is used to denote the stress which is also known as the engineering stress. To show that this is indeed the case, we denote the magnitude of the displacement gradient by ε = (ui,R · ui,R )1/2

(4.205)

We use the notation ε to indicate that this is a small quantity, and it should not be confused with the strain ε used in Chapter 3. The deformation gradient is FiR = δiR + ui,R = δiR + O(ε)

© 2005 by Chapman & Hall/CRC Press

(4.206)

194

Continuum Mechanics and Plasticity

where O(ε) indicates that the magnitude of this term has the order of ε. The determinant is |FiR | = det(δiR + ui,R ) = 1 + O(ε) + O(ε 2 ) + O(ε 3 )

(4.207)

ρ0 = ρ|FiR | = ρ(1 + O(ε) + O(ε 2 ) + O(ε 3 ))

(4.208)

Thus,

On the other hand the inverse deformation gradient F−1 is XR,i = δRi − uR,i = δRi − O(ε)

(4.209)

so that from (4.42) and (4.48) the Piola–Kirchhoff stresses are related to σij by (0)

TRi =

ρ0 ∂XR = (1 + O(ε) + · · · )(δRj − O(ε))σji σji ρ ∂xj

(4.210)

and

RS =

ρ0 ∂XR ∂XS = (1 + O(ε) + · · · )(δRj − O(ε))(δSk − O(ε))σjk (4.211) σjk ρ ∂xj ∂xk

In the limit, when ε → 0, we have (0)

TRi ≈ (δRj − O(ε))σji ≈ σRi

(4.212)

RS ≈ (δRj δSk + O(ε))σjk ≈ σRS

(4.213)

which show that the 1st and 2nd P–K stresses are indistinguishable from σij . The constitutive equation for inﬁnitesimal theory of elasticity at room temperature may be obtained by taking the strain-energy function W (εij ) in a quadratic form, that is, W = 12 Cijkl εij εkl

(4.214)

By differentiation of (4.214) with respect to εij , we obtain σij =

∂W = Cijkl εkl ∂εij

(4.215)

Equation (4.215) is known as the generalized Hooke’s law, where Cijkl is a fourth-rank tensor. If the material is isotropic, then Cijkl should be an isotropic tensor, that is, from (1.129) Cijkl = λδij δkl + µ(δik δjl + δil δjk )

© 2005 by Chapman & Hall/CRC Press

(4.216)

Conservation Laws and Constitutive Equation

195

By combining (4.215) and (4.216), we then obtain σij = λδij εkk + 2µεij

(4.217)

where λ and µ are Lamé constants. Note that the number of material constants has been reduced from 81 to 2. Equation (4.217) may be inverted to express strain in terms of stress. To this end, we make a contraction of (4.217) to get σii = 3λεii + 2µεii = (2µ + 3λ)εii

(4.218)

so that (4.218) may be solved for εii and substituted into (4.217) to obtain σij =

λσkk δij + 2µεij 2µ + 2λ

(4.219)

Finally, we rewrite (4.219) as 2µεij = σij −

λ σkk δij 3λ + 2µ

(4.220)

This is the equation that we wanted to derive.

4.9.2

Homogeneous Deformations

4.9.2.1 Hydrostatic stress Consider the strain

ε11 εij = 0 0

0 ε22 0

0 0 ε33

(4.221)

In the case of hydrostatic stress, ε11 = ε22 = ε33 = α. Substituting into (4.217), the stress is σij = (2µ + 3λ)αδij = −pδij

(4.222)

P = −(2µ + 3λ)α

(4.223)

Therefore,

and the volumetric strain is εkk = 3α =

© 2005 by Chapman & Hall/CRC Press

−3p −p σkk = = 3K 3K K

(4.224)

196

Continuum Mechanics and Plasticity

where K is the bulk modulus and σkk /3 is the mean stress. Thus, by use of (4.223), K=

−p −p 2 = =λ+ µ 3α (−3p)/(2µ + 3λ) 3

(4.225)

Note that since a hydrostatic pressure always causes the volume to decrease (α < 0), we have K > 0. In the case that p < 0, the volume expands and it is known as dilation. 4.9.2.2 Uniaxial tension When σ11 = σ22 = 0 and σ33 = 0, Hooke’s law reduces to σ11 = 2µε11 + λ(ε11 + ε22 + ε33 ) = 0 σ22 = 2µε22 + λ(ε11 + ε22 + ε33 ) = 0

(4.226)

σ33 = 2µε33 + λ(ε11 + ε22 + ε33 ) Comparing the ﬁrst two equations of (4.226), we ﬁnd λ (ε33 + 2ε22 ) 2µ

(4.227)

λ ε33 = −νε33 2(λ + µ)

(4.228)

ε11 = ε22 = − which may be solved to obtain ε11 = ε22 = − where ν=

1 λ 2λ+µ

(4.229)

is Poisson’s ratio. By substituting these expressions into the third equation of (4.226), we obtain σ33 = 2µε33 + λ(1 − 2ν)ε33 = (2µ + λ − 2νλ)ε33 λ2 µ(3λ + 2µ) = 2µ + λ − ε33 = ε33 = E ε33 λ+µ λ+µ

(4.230)

where E = µ(3λ + 2µ)/(λ + µ) is known as Young’s modulus. In an elastic material, E > 0 and ν > 0.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

197

4.9.2.3 Simple shear In the inﬁnitesimal deformation, simple shear does not give rise to normal stresses. The nonzero strain components are ε12 = ε21 only. From (4.217), the shear stress is σ12 = 2µε12

(4.231)

where µ > 0 is the shear modulus. The engineering shear strain is 2ε12 .

4.9.3

Boundary-Value Problems

In solving boundary-value problems of isothermal inﬁnitesimal elasticity, the fundamental equations are the equations of motion, σki,k + bi = ρ

D2 ui Dt2

(4.232)

the constitutive equations, σij = λδij εkk + 2µεij

(4.233)

and the strain–displacement relation, εij = 12 (ui,j = +uj,i )

(4.234)

There are three equations in (4.232), six equations in (4.233) and six equations in (4.234), and the unknowns are σij , εij , ui . We have 15 equations to solve for 15 unknowns. In ﬁnding the solution, the boundary conditions should be used. There are three types of boundary-value problems: the displacement boundary-value problems have ui speciﬁed on the boundary S; (n) the traction boundary-value problems have the stress vector ti speciﬁed on S; and the mixed boundary-value problems have ui speciﬁed on part of S (n) and ti speciﬁed on the remaining part of S. The surface traction is given, from (2.8), by (n)

ti

4.10

= σji nj

(2.8)

Hypoelasticity

Hypoelasticity is not elasticity, because the stress in hypoelasticity depends on the strain-path. This type of constitutive equation is popular in computational mechanics as it is of the rate-type. The rate-type equations have

© 2005 by Chapman & Hall/CRC Press

198

Continuum Mechanics and Plasticity

advantages over other types of equations due to the ease in numerical computation. We ﬁrst write the generalized Hooke’s law (4.217) of the inﬁnitesimal elasticity in the rate form as

σ˙ ij = 2µ˙εj + λδij ε˙ kk

(4.235)

and then inquire what the corresponding constitutive equation should be for ﬁnite deformation. We learned at the beginning of this chapter that objective rates need to be used in a constitutive equation. The Jaumann stress-rate is a popular objective stress rate and is used together with the rate of deformation tensor, so that an appropriate hypoelastic constitutive equation is written as σij∇ = 2µDij + λδij Dkk

(4.236)

A discussion using other objective stress-rates is given in Chapter 7 in connection with the study of plastic deformation. We discuss now a simple example using (4.236). Let us consider simple shear having the following equations x1 = X1 + 2ωt X2 , u1 = 2ωt X2 ,

0 [L] = 0 0

2ω 0 0

0 0 , 0

x2 = X2 ,

u2 = u3 = 0,

ω 0 0

0 [D] = ω 0

x3 = X3

(4.237)

ω = constant 0 0 , 0

0 [W ] = −ω 0

(4.238) ω 0 0

0 0 0 (4.239)

Substituting (4.239) into (4.236), we ﬁnd σij∇ = 2µDij

and

Dkk = 0

(4.240)

But the Jaumann rate is σ∇ =

Dσ − W · σ + σ · W = 2µD Dt

(4.241)

For the stress given by

σ11 [σ ] = σ12 0

© 2005 by Chapman & Hall/CRC Press

σ12 σ22 0

0 0 0

(4.242)

Conservation Laws and Constitutive Equation

199

we can compute the following matrices

−ωσ12 ωσ11 [σ ][W ] = −ωσ22 ωσ12 0 0 −ωσ12 −[W ][σ ] = ([σ ][W ])T = ωσ11 0

0 0 , 0 −ωσ22 ωσ12 0

0 0 0

(4.243)

Substituting (4.242) and (4.243) into (4.241), the component equations are dσ11 = 2ωσ12 , dt

dσ22 = −2ωσ12 , dt

dσ12 = 2µω − ω(σ11 − σ22 ) (4.244) dt

Note that D/Dt = d/dt in this homogeneous deformation. By differentiating (4.244c) with respect to t and making use of (4.244a,b), we obtain the ordinary differential equation d2 σ12 = −4ω2 σ12 dt2

(4.245)

The general solution of (4.245) is σ12 = A sin(2ωt) + B cos(2ωt) where A and B are constants. We deﬁne the shear strain by γ = during loading, the shear strain is

(4.246) t 0

D12 dt, and,

γ = 2ωt

(4.247)

Note that γ is not a component of a strain tensor. By taking the initial shear stress to be σ12 (t = 0) = 0, we ﬁnd from (4.246) that B = 0. Therefore, we obtain the following stress components σ12 = µ sin γ ,

σ11 = −σ22 = µ(1 − cos γ ),

other σij = 0

(4.248)

It can be seen from (4.248) that the shear and axial stresses oscillate with the increasing shear strain, and these are physically unacceptable with any real material. Nagtegall and de Jong [6] discussed this oscillatory behavior of the shear stress in his application of a plasticity model. The work triggered a longlasting investigation of objective stress rates by various investigators, and the subject is discussed further in Chapter 7 in connection with ﬁnite plasticity. Equations of (4.248) are plotted in Figure 4.12 with µ = 26.2 GPa, which is a typical value for cast high-purity aluminum.

© 2005 by Chapman & Hall/CRC Press

200

Continuum Mechanics and Plasticity Stress (MPa)

40 20 –4

2

–2

4

–20 –40 –60

12 22

FIGURE 4.12 Hypoelastic stress–strain curves by use of Jaumann stress rate.

References 1. Rivlin, R.S. and Ericksen, J.L., Stress–deformation relations for isotropic materials, J. Ration. Mech. Anal., 4, 323, 1955. 2. Green, A.E. and Adkins, T.E., Large Elastic Deformations, Oxford University Press, Oxford, 1960, 7. 3. Rivlin, R.S., Some topics in ﬁnite elasticity, in Proc. 1st Symp. Naval Structural Mech., Goodier, J.N. and Hoff, N.J., Eds., 1958, 169. 4. Rivlin, R.S. and Saunders, D.W., Large elastic deformations of isotropic materials VII. Experiments on the deformation of rubber, Phil. Trans. R. Soc. Lond., A243, 251, 1951. 5. Poynting, J.H., On pressure perpendicular to the shear planes in ﬁnite pure shears, and on the lengthening of loaded wires when twisted, Proc. R. Soc., A82, 546, 1909. 6. Nagtegall, J.C. and de Jon, J.E., Some aspects of non-isotropic workhardening in ﬁnite strain plasticity, in Proc. Workshop on Plasticity of Metals at Finite Strain: Theory, Experiment and Computation, Lee, E.H. and Mallet, R.L., Eds., Stanford University, 1981, 65.

Problems (1) Consider uniform extension of a material element followed by simple shearing. In the uniform extension along the X2 direction, a particle at X is displaced to X by X1 = β(t)X1 , X2 = α(t)X2 , X3 = β(t)X3

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

201

The subsequent simple shearing is expressed as x1 = X1 + 2η(t)X2 ,

x2 = X2 ,

x3 = X3

where 2η(t) is the shear strain after the uniform extension. Find the components of the 1st and 2nd P–K stresses expressed in terms of the Cauchy stress components. (2) For isotropic hyperelastic materials, show that the principal axes of the Cauchy stress and the left Cauchy–Green tensor coincide. (3) Consider a compressible isotropic hyperelastic material. For the deformation given by x1 = α(t)X1 ,

x2 = α(t)X2 ,

x3 = α(t)X3

discuss the corresponding state of stress. Obtain an expression for the stress vector and discuss the volume change of the material element. (4) Discuss the simple shear problem by means of Cauchy elasticity, that is, σij = χ0 δij + χ1 Bij + χ−1 B−1 ij where χ0 , χ1 , and χ−1 are functions of I1 , I2 , and I3 . (5) Find the state of stress in the biaxial compression of a cubic block discussed in Example 4.10, if the strain-energy function is given by W=

i

C1 (λ2i − 1) + C2

1 λ2i

−1

where C1 and C2 are constants and λi are the stretch ratios. (6) Find the state of stress in the simple torsion of a circular cylinder of incompressible hyperelastic material with length l and radius a. The deformation of this problem is expressed by x1 = (cos τ X3 )X1 − (sin τ X3 )X2 , x2 = (sin τ X3 )X1 + (cos τ X3 )X2 , x3 = X3 where τ is the angle of twist per unit length and is a constant.

© 2005 by Chapman & Hall/CRC Press

Part II

Continuum Theory of Plasticity Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (continuum) approach is still the practical approach for use in the simulation of engineering problems.

© 2005 by Chapman & Hall/CRC Press

5 Fundamentals of Continuum Plasticity

5.1

Introduction

A general description of plasticity is given in this chapter. Plastic deformation can be easily observed by stretching a thin copper wire. If we stretch a piece of copper wire beyond its elastic limit, then we observe a permanent change in length of the copper wire after the release of the load. This is because the wire is permanently elongated and has undergone a plastic deformation. The copper wire is very soft and easily stretched by a small force. The elastic limit of the material (copper) can be easily exceeded. In this onedimensional case, the experimental stress–strain curve for copper is sketched in Figure 5.1. We use this ﬁgure to illustrate properties and terminologies of plastic deformation. When the stress increases from O to A, the strain also has a proportional increase. The process of increasing the stress is known as loading. The initial yielding of the material occurs at A and the stress at this point is known as the yield stress and is denoted by σy . The yield stress is generally regarded as equal to the elastic limit, but the elastic limit and the proportional limit are experimentally indistinguishable for metals. Several deﬁnitions of yield stress have been proposed and they are discussed in Chapter 6. Should the stress be reduced from A back to O, we have an unloading process. OA is the elastic region and the Hooke’s law applies in this region. All strains within the elastic region are recovered upon unloading and are elastic strains. Point A is the ﬁrst point beyond which nonrecoverable strain occurs. This strain is permanent and is known as the plastic strain, which is either time-independent or time-dependent. In plasticity, we are interested in the time-independent nonrecoverable strain. The time-dependent nonrecoverable strain is related to creep. The curve OABE is the stress–strain curve for monotonic loading. The initial yielding of material occurs at A and yielding continues as the curve ABE is traversed. The strain at B is ε, which can be divided into the elastic ε e and plastic εp parts, where ε = εe + εp

(5.1) 205

© 2005 by Chapman & Hall/CRC Press

206

Continuum Mechanics and Plasticity

y

E

B

A

F Ο

p

e C

G

D FIGURE 5.1 Schematic stress–strain curve for Cu and Al.

The elastic and plastic strains for point B are shown in Figure 5.1. Curves BCD and EFG are unloading stress–strain curves. The initial part of the unloading curves is straight and the curves gradually bend over. In the ﬁgure, sections BC and EF are straight with slopes similar to that of section OA. Generally, for a good approximation, these slopes are assumed to be equal. But, experimental data show that the unloading slope depends on the strain level where the unloading begins to take place. Thus, EOA > ECB > EFE , that is, the slope is smaller if unloading occurs at a higher strain level. C and F are points of reverse yielding. Usually, the reverse yielding can occur on the compressive stress side as in point C, but as the strain at which unloading takes place gets higher, the reverse yielding occur on the tension side as in point F. The effect of the decrease in the yield stress in the reverse loading, that is, |σyC | < |σyB |, is known as the Bauschinger effect and it is an anisotropic hardening. The description of the stress–strain curve presented above is based on experimental observations and data. An enormous challenge in plasticity is to formulate a realistic mathematical model for describing the observed material behavior. The task is known as constitutive modeling and the end product is a constitutive model or a set of constitutive equations. Various theories using different approaches and points of views have been proposed to formulate constitutive equations for metallic materials. Theories have also been formulated based on dislocations and slips. Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (or continuum) approach is still the practical approach for use in the computational mechanics. Presently, there are great research efforts aiming to bridge the gap between mechanics at microscopic and continuum level. Some exciting results have already been reported and they provide input to the continuum theory of plasticity. Some of these inputs are discussed in Chapter 7 in connection with ﬁnite plasticity. In spite of the interest in plasticity at the microscopic level, the continuum theory is still the backbone for the study of plasticity.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

207

In this book, we discuss the continuum approach of plasticity. Most of our discussions are related to the plastic deformation of metals, although some may be applicable to other materials as well. In the study of plasticity, theories and experiments have gone hand-in-hand. Experimental results have led to the development of theories and theoretical studies have suggested new experiments. The ultimate goal is to develop a theory of plasticity that can be experimentally veriﬁed. Experimental results have been greatly inﬂuenced by the loading equipment and measuring technology. Problems associated with the loading equipment are the stiffness of the loading machine and the kind of the loading machine. Is it a dead-weight machine or is it a servo-controlled hydraulic testing system? Older data were gathered by use of dead-weight machine. Deadweight machines have an advantage in providing steady, well-controlled load increments and it can be used to obtain creep strains, but it cannot be used to execute a strain-controlled test program. Some dead-weight machines have cross-talks, that is, the axial load is inﬂuenced by the torsion load and vice versa in an axial–torsion test machine, resulting in inaccurate experimental results. Most commercially available servo-hydraulic machines have acceptable cross-talk level. An important advantage of the servo-hydraulic machines is that it is fully automated and it can execute either a strain-controlled or a stress-controlled test program. Due to the nature of the closed-loop servocontrolled machine, the data scatter to an extent which depends on the time interval of data acquisition. This data scatter may affect the accuracy of the data collected. Some examples that are sensitive to this data scatter are Young’s modulus of the stress–strain curve and yield stresses. These effects are further discussed in a later section. The strain can be measured by measuring the motion (displacement and rotation) of the cross-heads of the test machine. This method of measurement is, however, inﬂuenced by the stiffness of the machine and the shape of the specimens. Let L and φ, respectively, be the displacement and rotation of the cross-heads, r be the radius of a cylindrical specimen and L be the length of the specimen between the grips, then the axial strain ε and shear strain γ , respectively, are written as ε = L/L and γ = rφL. Since L includes the lengths of the enlarged gripping sections and the uniform gauge section of the specimen, the strains determined by use of the above expressions represent the average strains of the specimen and do not accurately represent the strains of the gauge section. It is the strains of the gauge section that are meaningful. The stiffness of the machine is not a factor, if we directly measure the strains in the gauge section of the specimen. Extensometers or strain gauges may be used to accomplish the job. Extensometers may be self-designed and is also available commercially. The resolution of extensometers is around 10−3 strain, but it can measure strains of up to about 15%. Extensometer for larger strains needs to be self-designed. Wu and Xu [1] built an axial–torsion extensometer that may be installed and clipped on the uniform gauge section of the specimen. Shear strains of up to 200% have been measured by Wu et al. [2]

© 2005 by Chapman & Hall/CRC Press

208

Continuum Mechanics and Plasticity

using this extensometer. Electrical-resistance strain gauges and strain rosettes are commercially available and they are easy to use. The resolution for this type of strain gauges is around 10−6 and it therefore provides much more accurate strain measurements than the extensometers. But, these gauges are limited to a strain of around 2% and either peel off or broken beyond 2% strain. A post-yield type strain gauge is available and it can measure axial strains of up to around 15%. No post-yield strain-rosettes are as yet commercially available. To design an experiment and collect valid data is a challenge and must be carefully pursued. The extension of one-dimensional plasticity into a multi-dimensional plasticity provides an even greater challenge both experimentally and theoretically. In the early development, two major schools of thought were developed; the ﬂow theory and the deformation theory. The deformation theory was proposed by Hencky in 1924 and the approach was used thereafter by Russian researchers. The Hencky equation is εij =

kσkk δij + ψsij 3

(5.2)

where k and ψ are scalars. We note that the total strain εij rather than the strain increment dεij is found from (5.2) and, therefore, the deformation theory is also known as the total strain theory. On the other hand, the ﬂow theory emphasizing the strain increment is also known as the incremental theory. The deformation theory is convenient for use, due to mathematical simplicity, in solving problems with proportional loading. The ﬁnal state of strain is determined by the ﬁnal state of stress. However, it is known that the equations of deformation theory are not suitable for nonproportional loading condition and the deformation theory will not be further pursued in this book. In this chapter we describe the fundamentals of plasticity from an experimentalist’s view point. The concepts of ﬂow theory is discussed in Chapter 6. The major concepts of ﬂow plasticity are: the yield surface, the ﬂow rule, the strain-hardening rule, and the loading–unloading conditions. Experimental evidence is presented together with the mathematical representations and assumptions of the theory are discussed. One of the major assumptions is the plastic incompressibility of metallic materials. Recent developments in plasticity are given in Chapter 7. It includes experimental and theoretical developments both for inﬁnitesimal and ﬁnite plasticity. Other developments, such as the endochronic theory, are discussed in Chapters 8 and 9. The author has been involved in the development and veriﬁcation of this theory, and a detailed account of the theory is given. The thermo-mechanical theory of internal state variables is ﬁrst presented in Chapter 8 and the presentation of the endochronic theory follows. The endochronic theory is an internal variables theory. Material anisotropy is an important topic of plasticity. The anisotropic properties of metal sheets are discussed in Chapter 10 and, in Chapters 11 and 12, we present a general theory of anisotropic plasticity. Since a square material element in the reference conﬁguration gets distorted by deformation,

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

209

curvilinear coordinates must be used and the stress and strain refer to this distorted element. In this way, we investigate the change in properties of the same material mass.

5.2

Some Basic Mechanical Tests

In this section, we discuss some basic experiments used to characterize the mechanical behavior of a material. They include the uniaxial tension test, uniaxial compression test, torsion test, and the creep test. These are onedimensional tests and aimed to produce axial and shear stress–strain curves and creep curves. They are very simple theoretically, but it is not so simple experimentally to obtain valid data. We refer to Bell [3] for a detailed account of experiments carried out during the ﬁrst half of the 20th century.

5.2.1

The Uniaxial Tension Test

Uniaxial tensile testing can be carried out quickly and easily and is used to measure the strength and ductility of materials. The specimens for tension test can be round or ﬂat specimens and they consist of enlarged end sections and a reduced gauge section. The round specimens can have threaded ends for gripping and the ﬂat specimens can either be with or without a pin-hole for connection to the load-train. The longer the gauge section is the more accurate the test results will be. The general shape of the loading stress–strain curve shown in Figure 5.1 is typical of those for aluminum, copper, brass, 304 stainless steel, and highstrength steels such as AISI 4142 steel in the small strain range, that is, when the strain is 50% before necking. Thinning of a sheet specimen can occur at a strain ·2 > ·1

·2 > ·1

(c)

T1

T2 T3

T3 > T2 > T1

FIGURE 5.9 (a) Schematic constant strain-rate stress–strain curves, (b) constant strain-rate stress–strain curves for mild steel, (c) the effect of temperature.

A

A

B C

O

A

FIGURE 5.10 Loading stress–strain curve, creep, and stress relaxation.

Some fundamental concepts of strain-rate effect are constant strain-rate stress–strain curves as previously discussed, creep, and stress relaxation. Creep is the deformation developed as time elapses when the applied stress is kept constant. On the other hand, when the strain is kept constant, the stress relaxes with time. In Figure 5.10, OA shows the loading stress–strain curve; AB shows that the strain creeps from A to B while the stress is kept constant at σA ; and AC shows that the stress relaxes from A to C while the strain is kept constant at εA . A typical creep curve is a plot of strain against time and it is divided into three stages: the primary creep, the secondary creep,

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

227

D B

C

A

O

t

FIGURE 5.11 A schematic creep curve with three stages.

and the tertiary creep, as shown in Figure 5.11. The primary creep (also known as the transient creep) (AB) occurs at the beginning of the creep process. During this stage, the creep rate decreases continually. The creep rate remains nearly constant in the secondary (or steady state) creep stage (BC), and the creep rate increases continually until rupture during the tertiary creep stage (CD). It is convenient to separate the creep into three stages. However, no observations are available that show creep to be completely separated into three independent stages. It takes a long time to reach the tertiary stage; tertiary stage begins after 1940 h of creep, for instance, for an austenitic stainless steel tested at 704◦ C under a stress of 90.9 MPa (13,200 psi) [23]. The creep curves are dependent on the hold stresses. The higher the hold stress, the larger is the creep strain. Creep tests conducted at constant load or constant stress also give different creep curves. In the past (before about 1980), plastic deformation and creep were investigated separately. Experiment to determine plastic behavior was performed by use of screw-driven universal testing machines and creep experiment was conducted by dead load machines. An accurate control of rate of loading or rate of straining was difﬁcult in both cases. This method of experimental investigation gave rise to separate theories for plastic deformation and creep behavior. In this manner, the inelastic strain consists of a time-independent plastic strain term and a time-dependent creep strain term; these terms are calculated using plasticity and creep theories, respectively. Recently (after about 1980), new type servo-controlled testing equipment permits an accurate control of rate of loading or straining under quasi-static condition. It provides the means of recording the nonlinear, inelastic behavior of materials in detail and with great accuracy. The machine is so powerful that interactions between plasticity and creep can also be investigated. In this connection, we are interested in the primary and secondary creep stages. It is difﬁcult to draw a line between the two stages as previously mentioned and we will show continuous creep curves. Some interaction phenomena that have been reported are: the cyclic hardening or softening with hold time;

© 2005 by Chapman & Hall/CRC Press

228

Continuum Mechanics and Plasticity

the effect of creep prestrain on the subsequent plastic behavior; and the effect of plastic strain on the subsequent creep behavior. Corum et al. [24] showed that the stress amplitude in the cyclic tension–compression tests with a constant strain amplitude was enhanced by the preceding creep for AISI Type 304 stainless steel. Ikegami and Niitsu [25] found that SUS 304 stainless steel hardens in the direction of the preloading not only by plastic strain but also by creep strain. The hardening by creep is nearly equal to that by plastic strain. Wu and Ho [26] investigated strain hardening of 304 stainless steel by creep and found that the material hardened by creep is the same as that hardened by plastic deformation. Kujawski et al. [27], Wu and Yao [28], Wu and Ho [29], and Xia and Ellyin [30] observed that the creep curves are different even at the same holding stress but for different strain- or stress-rate loading histories prior to creep. In order to describe the aforementioned plasticity–creep interaction, recent efforts in material constitutive relation lean towards a uniﬁed theory for plasticity and creep. A fundamental issue of the creep test is the large range of data scatter. Some of the scatter may be attributed to the material inhomogeneities, but there are two other important factors contributing to the scatter. One factor is the test system misalignment and the other is the negligence of the pre-loading stage in a creep test by the investigators. These two factors are further explained. The misalignment in creep was investigated by Penny and Leckie [4] and Hayhurst [31]. These research workers generally agreed that data scatter in creep testing could be partially attributed to specimen alignment. Poor specimen alignment could result in bending stress (or strain) superimposed on the required mean axial stress (or strain). This bending stress (or strain) could be high enough to cause premature failure in brittle materials; in ductile materials, plastic deformation could occur and reduce the bending stress (or strain). Analyses of misalignment were presented by these investigators. The results show that the creep curves scatter due to eccentric loading. More signiﬁcantly, these analyses predicted that the scatter would increase with the creep time. The result of Wu and Wang [32] does not support all of the above assertions. Wu and Wang [32] considered the effect of pull-rods and the symmetric case of misalignment shown in Figure 5.3. The symmetric case is the most severe case of misalignment as discussed in [5]. It was pointed out in [32] that the following assumptions and/or conditions used by [4] and [31] are not realistic: (1) the applied load P is linearly related to the end moment M; (2) dP/dt = dM/dt = 0; (3) the neutral axis of the specimen is ﬁxed; and (4) the absence of pull-rod effect. The analysis of Wu and Wang [32] relaxed all of the aforementioned assumptions and led to different results as compared with [4] and [31]. While the numerical results of [32] show that the errors induced by the test system misalignment are signiﬁcant in the creep test, these errors will diminish with time. Thus, the most severe effect of misalignment occurs at the beginning of the creep test. Creep tests conducted with long pull-rods and large initial strain level (high creep stress) will tend to minimize the effect of misalignment.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

229

Another factor that is contributing to the scatter of creep data is the negligence of the preloading stage in a creep test. Due to the nature of dead load creep machines, the strain rate of the preloading stage in a traditional creep test is neither observable nor recordable. The way that the load (weight) is applied greatly affects the creep strain. Wu and Ho [29] conducted creep tests by use of a servo-controlled materials test system, and investigated the effect of the preloading stage on the subsequent creep. Two sets of test histories were used. One had a constant strain-rate preloading and the other had a constant stress-rate preloading. In the case with constant strain-rate preloading, the specimen was pulled in the strain-control mode while the computer monitored the strain and stress magnitude. The strain-rates were set at 2 × 10−6 , 10−5 , 10−4 , and 10−3 s−1 . As soon as the stress magnitude reached the preset creep holding stress, the loading process stopped. The test system was programmed to switch to the load-control mode instantaneously and then kept the stress at this constant magnitude, while the creep strain was being recorded. In the case with constant stress-rate preloading, the test was straightforward without control mode switching. The tests were performed under stress control at constant stress-rates of 2.07 and 20.7 MPa/s. As the stress reached the preset value, the creep process began. Each test result to be discussed was the average of two specimens. Most results were very consistent except for the case of constant strain-rate loading at 10−5 s−1 , where data scatter was apparent. A third test was conducted for this case and the result shown is the average of three tests. Two remarks can be made from the strain–time proﬁles of the whole creep process (the loading stage and the creep stage) shown in Figure 5.12, in which the starting point of the creep stage is marked by *. First, the proﬁles conﬁrm the constant strain-rate control of each curve prior to reaching the hold stress. Second, the proﬁles show that the initial creep strain rates are indeed a continuation of the preloading strain rates. Therefore, the initial creep strain rate of creep tests with strain-controlled preloading is known. Figure 5.13 shows the creep curves of various constant strain-rate preloading at the same holding stress of 206.7 MPa (30 ksi). For constant stress-rate preloading, the initial creep strain rate is also determined at the end of the loading stage. Thus, in the discussion of the creep stage, the initial creep rate is regarded as a known value. Figure 5.14 shows the strain–time proﬁles of the creep tests with constant stress-rate preloading. The starting points of the creep stage are marked by ∗ in the ﬁgure. It is seen that, during the preloading stage, the strain rate is constant in the elastic range and increases rapidly during elastic–plastic transition. The ﬁgure also shows that the initial creep strain rate is a continuation of the preloading strain rate. Figure 5.15 shows the creep curves for two creep tests with preloadings of two different constant stress rates. The hold stress for both tests was 206.7 MPa (30 ksi), same as the hold stress for the creep tests shown in Figure 5.13. In the elastic region, stress-rates of 2.07 and 20.7 MPa/s correspond to strain-rates of 1 × 10−5 and 1 × 10−4 s−1 , respectively. Because the initial creep rate of the creep test with faster stress-rate preloading is large, the corresponding creep

© 2005 by Chapman & Hall/CRC Press

230

Continuum Mechanics and Plasticity 2.5 1.e – 4 1.e – 5

2.0

2.e – 6 Total Strain (%)

1.e – 3 1.5

1.0

0.5

0

–0.5 0

50

100

150

200

Time (min)

Creep Strain (%)

FIGURE 5.12 Strain–time proﬁles of creep tests with various constant strain-rate preloading (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

–3

1.2

10

1

10

–4

0.8 –5

0.6

10

0.4

= 2 × 10

–6

0.2 10

20

30 40 Time (min)

50

60

FIGURE 5.13 Creep curves of various constant strain-rate preloading at the same hold stress (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

strain is larger than that of the creep test with a slower stress-rate preloading. Comparing creep curves of Figure 5.13 and Figure 5.15 with the same preloading strain-rate in the elastic region and having the same hold stress, the creep strains of constant stress-rate preloading approximately double those of constant strain-rate preloading. We may conclude that the preloading stage greatly affects the subsequent creep strain and that the traditional creep test using a dead load machine is vulnerable to data scatter, because neither the strain- nor the stress-rate of the loading stage can be controlled.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

231

2.5

Total Strain (%)

2.0 1.5 1.0 20.7 MPa/s 2.07 MPa/s

0.5 0

–0.5 0

10

20

30 40 Time (min)

50

60

70

FIGURE 5.14 Strain–time proﬁles of creep tests with constant stress-rate preloading (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

Creep Strain (%)

20.7 MPa/s

1.5 2.07 MPa/s

1 0.5

10

20

30 40 Time (min)

50

60

FIGURE 5.15 Creep curves of two constant stress-rate preloading at the same hold stress (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

5.3

Modeling the Stress–Strain Curve

For the purpose of applications and further theoretical studies, it is useful to develop a mathematical model for the one-dimensional stress–strain curve OABE shown in Figure 5.1. This is a generic stress–strain curve, it can be the curve for tension, compression, or shear. In 1909, Ludwik [33] proposed a stress–strain relationship to be used when the deformation was sufﬁciently

© 2005 by Chapman & Hall/CRC Press

232

Continuum Mechanics and Plasticity (a)

n = 0.5 n = 0.4 n = 0.3 n = 0.2 n = 0.1 n=0

2

/K

1.5 1 0.5

1

2

3

4

(b)

2.0 m=3 1.5

/y

m=5 m=9 m = 14 m = 30

1.0

0.5

1.0

2.0 3.0 /y

4.0

FIGURE 5.16 (a) The Ludwik equation, (b) the Ramberg–Osgood equation.

large so that the elastic strain could be neglected. The Ludwik equation is σ = Kεn

(5.37)

where K is a strength coefﬁcient and n is a strain-hardening exponent usually lying between 0 and 0.5. The equation predicts a zero initial stress and an inﬁnite initial slope, except for n = 0 which represents a rigid perfectly plastic material without strain-hardening. The higher the value of n, the more pronounced is the strain-hardening characteristic of the material. The Ludwik equation is plotted in Figure 5.16(a) for n = 0, 0.1, 0.2, 0.3, 0.4, and 0.5. If this equation is used to describe the plastic behavior and we combine the equation with Hooke’s law, which is used to describe the elastic behavior, the resulting equation can be used to describe the total material behavior. Writing the total strain as the sum of elastic and plastic parts, we obtain ε = εe + εp =

© 2005 by Chapman & Hall/CRC Press

σ σ 1/n + E K

(5.38)

Fundamentals of Continuum Plasticity

233

This equation, known as the Ramberg–Osgood Equation [34], is used by many investigators to express the monotonic loading curve of strain-hardening materials, especially ones without a sharply deﬁned yield stress. For a large number of metals, if the true stress is plotted versus the true plastic strain, a straight line results on a log–log plot and equation (5.38) proves useful. We rewrite (5.38) as ε σ = +α εy σy

σ σy

m (5.39)

where α=

E(σy )m−1 Km

and

m=

1 n

(5.40)

and σy and εy are the yield stress and yield strain, respectively, and related by σy = Eεy ; m is a hardening exponent; and α is a constant. Equation (5.38) is plotted in Figure 5.16(b) for α = 3/7 and m = 3, 5, 9, 14, and ∞. Note that (5.39) has three parameters. Other models have been proposed in the literature, but they will not be discussed here. Generally, the models describe similar curves using different mathematical expressions. Instead, we give some remarks related to the stress–strain curves in the large strain range. Many investigators specify that their equations relate the true stress to the true strain. The true strain is well deﬁned and the deﬁnition of true strain or logarithmic strain ε log has been discussed in Section 3.10. It may be shown from (3.139) that true strain is related to the engineering strain εeng by εlog = ln(1 + ε eng )

(5.41)

The true stress (or the Cauchy stress) is also well deﬁned and it is related to the nominal stress (or the 1st P–K stress) by (4.42). In the case of uniaxial stress for isotropic materials, the deformation gradient and stress components are

λ [F] = 0 0

0 λ2 0

0 0 , λ2

σ [σ ] = 0 0

0 0 0

0 0 , 0

s [T (0) ] = 0 0

0 0 0

0 0 0 (5.42)

Assuming that the material is incompressible at large strain, the Jacobian of the transformation is J = det F = λλ22 = 1

© 2005 by Chapman & Hall/CRC Press

(5.43)

234

Continuum Mechanics and Plasticity

Substituting (5.42) and (5.43) into (4.42), we obtain s=

σ = σ exp(−εlog ) λ

(5.44)

λ = exp(εlog )

(5.45)

where

Equation (5.44) has been used to convert the stress–strain curve expressed in terms of the true stress σ into that expressed in terms of the nominal stress and vice versa. In the tension test, the nominal stress is easily determined, because the initial cross-sectional area of the specimen is known. In this case, (5.44) is used to convert the nominal stress into the true stress. Both stress–strain curves are shown in Figure 5.17(a). Recently, some investigators have used diametral extensometers to measure the diametral strains in the cylindrical tension specimens. These diametral strains are then converted to the longitudinal strains based on a constant volume assumption. Let the volume be V = A0 l0 = Al, where A denotes the cross-sectional area and l the length of the specimen. The subscript 0 denotes the undeformed condition. If the volume remains constant, the differentiation of the above equation leads to dε

log

dA dl =− = l A

or

ε

log

A0 = ln A

(5.46)

The diametral strain is related to the change of area. The reduction of area deﬁned by (A0 − A)/A0 is often used. However, we need to remember that this approach is based on the constant volume assumption and it is a good approximation when the strain is large. In the compression test, the specimen is repeatedly remachined. The stress thus obtained is close to the true stress. We then use (5.44) to convert the true stress into the nominal stress. In doing so, we remark that the strain ε log is negative in compression. The stress–strain curves for compression are shown in Figure 5.17(b) plotting against the absolute value of the true strain.

5.4

The Effects of Hydrostatic Pressure

The hydrostatic pressure plays a signiﬁcant role in the formulation of a modern theory of plasticity. It has been assumed by many researchers that plastic yielding of metals is independent of superimposed hydrostatic pressure and that metals are plastically incompressible. In this section, we examine the experimental ﬁndings that have been reported in the literature so that the validity of the aforementioned assumptions can be assessed. We would like

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

235

(a) 2.5

Stress

2 1.5

s

1 0.5 0.2

0.4

0.6

0.8

1.0

log

(b) 2.5 s

Stress

2 1.5

1 0.5 0.2

0.4

0.6 log

0.8

1.0

FIGURE 5.17 Stress–strain curve expressed in two stress measures, (a) tensile and (b) compression.

to mention that the dependence of the yield stress and the compressibility of material on the hydrostatic pressure are well recognized for such porous materials as geotechnical materials and is not be discussed in this section (see Chapter 9 for discussion). Bridgman published a large volume of papers related to high hydrostatic pressure. The experiments related to the studies of large plastic ﬂow under the effect of hydrostatic pressure are well summarized in Bridgman [9]. From the many solids studied, the “absolute compressibility” of the material is given from [3, p. 493] by −

V = a p − b p2 V0

(5.47)

where p is the hydrostatic pressure measured in kgf/cm2 (1 kgf/cm2 = 98.1 kPa), V the volume change, V0 the initial volume at atmospheric pressure, and a and b are constants determined from experiments, for example, a = 5.826 × 10−7 and b = 0.8 × 10−12 for iron. We note that the absolute compressibility expressed by (5.47) is a volumetric strain and would like to mention a special note by Bell [3, p. 494] that Bridgman measured the change

© 2005 by Chapman & Hall/CRC Press

236

Continuum Mechanics and Plasticity

in length in a single direction from which, assuming isotropy, he computed the change of volume. In the tension of steel under hydrostatic pressure, Bridgman [9, p. 49] measured the change in length of the specimen and by the assumption of volume constancy he determined the area reduction of the neck in the tension specimen. He found that the ﬂow stress and the stress at maximum load increase almost linearly with pressure for pressure up to 2,800 MPa (400,000 psi) for various heat treatment of a steel, Bridgman [9, p. 69–70]. Bridgman [9, p. 195] conducted uniaxial compression test using specimens of various metals to determine plastic volume change. No hydrostatic pressure was applied in this series of tests. He used a dilatometer apparatus for determining the change of volume of the specimen during the test. He argued for the superiority of a direct measurement (by use of dilatometer) of the volume change as compared with its indirect determination from measurements of the change of longitudinal and lateral dimensions. Bridgman considered a cylinder of mild steel plastically shortened to 0.85 its initial length by an axial load of 689 MPa (100 ksi), and he compared the radius of the cylinder under two conditions: assuming no change of volume and assuming the full elastic change of volume corresponding to this stress. He found that the radius in the two cases differs only by 0.07%, which is a difﬁcult task for measurement. Bridgman did not compare the circumferential strain, however. If he did, he would have found that the difference is 0.94%, and the circumferential strains are 0.08465 and 0.08545, respectively, which is not a difﬁcult task for today’s measurement technology. Bridgman immersed the specimen undergoing plastic deformation in a dilatometer, which was ﬁlled with a liquid and provided with a capillary open to the atmosphere in which the liquid meniscus moved in response to changes in volume of the contents of the dilatometer. Of the materials examined under compression, negative plastic volumetric strains were shown by annealed high-carbon steel, 303 stainless steel, copper, and hard-drawn brass, and the opposite effect, a positive plastic volumetric strain, was shown by mild steel and iron. With these differences, the plastic volumetric strains were small, however, and most volume changes were recoverable on release of stress. Examples were: the plastic volumetric strain for 1035 steel was 0.0001 for an axial strain of 0.02; it was 0.00012 for 303 stainless steel for an axial strain of 0.135; and it was 0.00015 for high-carbon steel for an axial strain of 0.14. Crossland [35] and Hu [36] found that the yield stress in torsion was sensitive to the presence of hydrostatic pressure up to 280 MPa (40 ksi). Crossland found that the upper yield stress of mild steel decreased by 10% and Hu found that it decreased by 6.5% over the same range of hydrostatic pressure. Permanent volume expansion was observed for 4310 and 4330 steels by Spitzig et al. [7]. These authors determined the density at the uniform gauge section of the specimen. Measurements were made both before and after straining specimens up to 4% plastic strain, and, therefore, these were permanent volume changes. Additional volume-change measurements were made during deformation on several tension specimens with rosette strain

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

237

gauges. It was found that tensile and compressive testing under hydrostatic pressure up to 1100 MPa (160 ksi) raises the stress–strain curve by about 6.5%, but does not signiﬁcantly affect the work-hardening characteristics. The plastic volumetric strain increased proportionally with the axial strain, and it was about 2 × 10−4 when the axial strain was 0.04. Volume-change measurements made from the strain gauges were similar in magnitude to those obtained from the density measurements. For the hydrostatic pressure of 1400 MPa (200 ksi) the elastic volumetric strain is 8.78×10−3 and the plastic volumetric strain is only 2% of this amount. It may be concluded that the yield stress of metallic materials depends on superimposed hydrostatic pressure. The yield stress in tension, compression, or torsion may increase or decrease with pressure depending on material tested. Further investigation to experimentally quantify this effect is warranted. However, for a ﬁrst approximation, the assumption that plastic yielding of metals is independent of superimposed hydrostatic pressure is reasonable. We are convinced that the plastic volumetric strain is small compared to the elastic volumetric strain. Therefore, the assumption of plastic incompressibility is well established. The assumption of plastic incompressibility is expressed in terms of the increments of the plastic strain as p

p

p

p

dεkk = dε11 + dε22 + dε33 = 0

5.5 5.5.1

(5.48)

Torsion Test in the Large Strain Range Introduction

Torsion tests in the large strain range provide results that are useful in the development and veriﬁcation of microstructure-based and phenomenological constitutive models of crystalline solid. The test is quite complex since, in addition to shear stress and shear strain, the axial and hoop strains and the axial stress are also important, making torsion test a multi-axial test. There are two end-conditions in the torsion test: the ﬁxed-end and the free-end torsion. In the ﬁxed-end torsion, the length change of the specimen is prevented, and, because of this, axial stress is developed during torsion. On the other hand, the length change is permitted in the free-end torsion, but the axial stress is zero during torsion. The existence of axial stress or axial strain in the torsion test is generally known as the axial effect. Some torsion tests are cited as: Poynting [37], Swift [38], Hughes [39], Hodierne [40], Ronay [41,42], Baily et al. [43], Billington [44], Lindholm et al. [45], Van Arsdale et al. [46], Montheillet et al. [47], Wu et al. [2,48], Lipkin and Lowe [49], White et al. [50], Weerasooriya and Swanson [51], Toth et al. [52], and Miller and McDowell [53]. Several problems related to such torsion tests need to be addressed. If these problems are not carefully considered, then the validity of test results may be questioned. The problems are associated with the homogeneity of the

© 2005 by Chapman & Hall/CRC Press

238

Continuum Mechanics and Plasticity

material, the strain measurement, the specimen geometry, and the determination of the shear stress–strain curve from the experimental torque versus angle of twist curve. These problems have been discussed in [2] and the following discussions are based on [2]. (1) The material homogeneity: If the material is not homogeneous, nonuniform deformation will occur, leading to regions that remain almost undeformed while plastic deformation occurs in the remaining part of the specimen. The strain concentration will lead to an early development of shear band localization in the specimen. This is a very serious problem, especially when long gauge-length specimens are used. In the research of [2], well controlled, homogeneous material was supplied by a material manufacturer and macroscopically uniform plastic deformation (no apparent regions of strain concentration were observed by eye inspection after the test) was obtained in all specimens tested. (2) The strain measurement: An important problem associated with the torsion test and the combined axial–torsion test is the strain measurement. A transducer that measures and controls normal and shear strains in the large strain range is not generally available. Almost all experimental results reported in the literature use the relative motion between the grips to compute the axial and shear strains. This method does not lead to accurate strain measurements due to the geometry of the specimen, which has enlarged ends. An axial–torsional extensometer has been designed and built by Wu and Xu [1], see Figure 5.18. This extensometer measures strains in the gauge section of the solid shaft or tubular specimens. Speciﬁcations of the extensometer have been determined in terms of the linearity, cross-talk, and hysteresis, and have been reported in Wu and Xu [1]. In particular, the cross-talk between axial and shear channels is 150◦ C (300◦ F), which is the upper temperature limit for the LVDTs and RVDTs of the extensometer. For higher temperature tests, a different method of calibration must be used and specimens were required in this procedure. Calibration curves were determined at room and 150◦ C temperatures. It was then assumed that these curves were still valid at higher temperatures. A total of four short specimens of cast aluminum were used for the calibration tests in free- and ﬁxed-end torsion conditions. Figure 5.20(c) shows the calibration curves plotting the grips rotation of the test machine against the relative rotation within the gauge length, measured by the extensometer, of a short specimen tested in free-end torsion at two different temperatures. It is seen that no noticeable differences can be found between the two curves. This curve describes the geometrical characteristic of the specimen and shows that the relation has not been affected by temperature. Similar calibration curves for short specimen subjected to ﬁxed-end torsion have also been obtained. Again, temperature does not have a noticeable inﬂuence on the calibration curve. The calibration curves plotting the stroke of the test system versus the axial extension within the gauge length of a specimen have also been determined and it has been found that the curve is not affected by test temperature either. An assumption is then made that these curves remain unchanged at higher temperatures at 205◦ C (400◦ F) and 315◦ C (600◦ F), so that they may be used to convert the stroke and rotation readings recorded during tests at 205◦ C and 315◦ C into axial and shear strains, respectively. At these temperatures, due to an added heating element, about 3 to 4 h of heating time were needed for the environmental chamber to reach a steady uniform temperature. 5.5.2.3 The hoop strain measurement There are rarely any experimental data reported concerning the hoop strain. Baily et al. [43], recorded the hoop strain by taking readings of ﬁnal diameter for nine specimens, which were tested at different levels of shear strain. However, a plug was used during the torsion tests, which might have restricted the diametral change. Although the diameter reduction was observed by many investigators (Swift [38], Freudenthal and Ronay [56], Ronay [41]) no reliably recorded data were taken either during the tests or after the tests. Data of diameter can provide important information as much as the axial extension does. In [2], the hoop strain was determined by accurately measuring the diameter change during torsion. A ring was attached to the middle of the gauge section of the specimen by use of four, equally spaced (90◦ apart), spring-loaded pins. Two pins located at the opposite side of the diameter of the specimen

© 2005 by Chapman & Hall/CRC Press

246

Continuum Mechanics and Plasticity

formed a pair. The displacement of each pin was measured by a LVDT and the readings for each pair of pins were averaged. This data and that obtained from the second pair of pins were then averaged to provide the data for diametral change during torsion. In order to conﬁrm the measured diametral change, a micrometer with 0.0025 mm (0.0001 in.) accuracy was used to measure the diameter. The measurement was taken at upper, middle, and lower cross-sections within the gauge section after each test run at room temperature. Several test runs were conducted, one after the other, so that a shear strain of 200% was obtained. After the tests, the specimens were cut in the middle section and the diameters were again measured. The data were consistent with the LVDT readings. The hoop strain was then computed by dividing the diametral change by the initial diameter. In the tests for measuring the diametral change, the axial and shear strains were determined by the stroke and rotation, respectively, of the test machine. These readings were then converted into axial and shear strains by use of a set of calibration curves, one of which is shown in Figure 5.20(c).

5.5.3

Experimental Results and Discussions

Experimental results of [2] were analyzed and presented in terms of true shear stress–strain curve, axial strain, hoop strain, and axial stress. The difference between the cast and the extruded aluminum and the effect of test temperature are discussed in each item. Finally, the effect of specimen geometry is also discussed. 5.5.3.1 The true shear stress–strain curve Raw experimental data in terms of torque versus angle of twist curves were analyzed by the modiﬁed Nadai method presented by Wu et al. [20]. The method accounts for length change in free-end torsion, and it is a method to determine the true shear stress–strain curve without measurement of radial and hoop strains. The true shear stress is deﬁned in Wu et al. [20,22] based on the current cross-section of the specimen. The method of Wu et al. [20,22] is discussed in Section 5.5.4. The axial strain was computed simply by dividing the axial extension by the initial gauge length. It was a good approximation, since the axial extension was a small deformation. In the case of ﬁxed-end torsion, Nadai’s method [6] was used, since there was no axial length change. Figure 5.21 shows the shear stress–strain curves for extruded aluminum at room and 150◦ C (300◦ F) temperatures. It is seen that the stress is lower at 150◦ C and that the shear stress–strain curve of ﬁxed-end torsion is slightly higher than that for free-end torsion. This difference is due to the analysis (Wu et al. [20]) which assumes that the hoop strain and axial strain ratio is 0.5. According to the experimental results to be presented later in this section, this ratio is much greater than 0.5. An analysis by use of [22] with

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

247

60

Shear Stress (MPa)

50 40 30

Fixed-end (Short) Free-end (Short) Free-end (Long) Fixed-end (Short 300° F) Free-end (Short 300° F)

20 10 0 0

25

50

125 75 100 Shear Strain (%)

150

175

FIGURE 5.21 Shear stress–strain curves for extruded aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

80

Fixed-end (Short) Free-end (Short) Free-end (Long) Free-end (Medium) Room Temperature

Shear Stress (MPa)

60

Fixed-end (Short 300° F) Free-end (Short 300° F)

40 Fixed-end (Short 400° F) Free-end (Short 400° F)

20

Free-end (Short 600° F) Fixed-end (Short 600° F)

0 0

50

100 Shear Strain (%)

150

200

FIGURE 5.22 Shear stress–strain curves for cast aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

the hoop strain and axial strain ratio equal to 0.9 would make the two curves coincide. This correction has been made for curves in Figure 5.22 which are for cast aluminum. It sufﬁces to mention that the curves for ﬁxed-end torsion in Figure 5.21 are the true stress–strain curves.

© 2005 by Chapman & Hall/CRC Press

248

Continuum Mechanics and Plasticity 150

Mises Stress (MPa)

Cast P0815 Aluminum ATC Compression Test

100

Extruded P0815 Aluminum Tabular Specimen Torsion 50

0

Cast P0815 Aluminum Tabular Specimen Torsion

0.0

0.2

0.4 Effective Strain

0.6

0.8

FIGURE 5.23 Comparison of mises stress obtained from torsion and compression (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

The curves of Figure 5.22 were obtained from free- and ﬁxed-end torsion tests at room, 150◦ C (300◦ F), 205◦ C (400◦ F), and 315◦ C (600◦ F) temperatures using long, medium, or short specimens. It is seen that these curves are strongly affected by temperature. The higher the temperature is, the lower is the shear stress–strain curve. Short specimens were tested at all four temperatures. The curves of those specimens under ﬁxed- and free-end condition are indistinguishable at all temperature levels. Long and medium gauge length specimens were also used in the room temperature testing under free-end condition. It is seen that the curves at room temperature for specimens of all gauge lengths are very close to each other. Figure 5.23 shows the experimental data of cast and extruded aluminum from the present torsion tests compared to the compression tests obtained by Wang et al. [57]. Note that there is an interruption in the compression curve due to unloading and specimen remachining. The curves are plotted in the form of Mises stress versus effective strain. (The Mises stress is deﬁned based on the Mises yield criterion, which is discussed in Chapter 6 in connection with the ﬂow theory of plasticity; and the effective strain is deﬁned based on the second invariant of the strain tensor.) It is seen that the torsion curve for extruded aluminum, which has prestrain texture, lies higher than that for cast aluminum. Furthermore, the ﬁgure shows that the mises stress cannot be used to obtain a uniﬁed stress–strain curve for cast aluminum, because the stress for compression test is higher than that for torsion test. This is so because the two tests lead to different textures. 5.5.3.2 The axial strain The axial effect takes the form of length change during free-end torsion. Figure 5.24 summarizes test data for axial extension versus shear strain for

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

249

4 Extruded P0815 Aluminum Long and Short Specimens Axial Strain (%)

3

2

1 Cast P0815 Aluminum (1/8⬙, 1/4⬙ and Solid)

0 0

30

60

90

120

150

Shear Strain (%) FIGURE 5.24 Axial strain in free-end torsion for cast and extruded aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

cast and extruded aluminum. The effect of specimen geometry is signiﬁcant and is discussed in a subsequent section. For extruded aluminum, the axial extension starts to increase at the early stage of torsion test and continues to increase thereafter. The notation EAL denotes extruded aluminum with long specimen and EAS denotes extruded aluminum with short specimen. The wall-thickness was 6.4 mm for both curves. The slopes of axial strain curves decrease slightly at large shear strain level. For cast aluminum, the rate of axial extension is very small when the shear strain is 50%. In the ﬁgure, CA1/8 denotes cast aluminum tubular specimen with 3.2 mm (1/8 in.) wall-thickness and medium gauge length; CA1/4 denotes cast aluminum tubular specimen with 6.4 mm (1/4 in.) wall-thickness and long gauge length; and CASOL denotes cast aluminum solid shaft specimen. This ﬁgure shows that the development of axial effect in the cast aluminum was delayed by a shear strain of approximately 50% when compared with the extruded aluminum. Figure 5.25 shows that the test temperature does not have a signiﬁcant inﬂuence on the axial extension for cast aluminum. In the case of extruded aluminum (not shown in the ﬁgure), the axial extension curve at room temperature is slightly higher than that at 150◦ C (300◦ F), but they almost coincide. This ﬁnding does not agree with the assertion [41] that a higher temperature would give rise to a larger axial extension, and it is not consistent with the temperature effect observed in the axial stress developed during ﬁxed-end torsion test discussed in the next subsection. Different textures are developed at different test temperatures and they can cause different amounts of length

© 2005 by Chapman & Hall/CRC Press

250

Continuum Mechanics and Plasticity 2.0

300° F (Short)

Axial Strain (%)

1.5

400° F (Short) 600° F (Short)

1.0

0.5

0.0 0

25

50 75 Shear Strain (%)

100

125

FIGURE 5.25 Axial strain in free-end torsion at elevated temperature (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

change. It is believed that the specimen geometry effect is responsible for this inconsistency. The geometry effect is important in the free-end torsion test and not as important in the ﬁxed-end torsion test. Therefore, it is believed that the observed dependence of the axial stress on temperature is a true effect. From this viewpoint, one can then infer that a temperature effect should also exist in the length change, but it should be further investigated. 5.5.3.3 The hoop strain For a few specimens where the outer diameter change was measured during free-end torsion, the hoop strain was computed from the diametral change. Figure 5.26 shows the axial and hoop strains plotted against the shear strain for cast and extruded aluminum at room temperature. Two long specimens of extruded aluminum (marked “textured” in the ﬁgure) were tested and the results are very consistent. The axial strain was about 5.5–6% and the hoop strain was about 4.0–4.5% when the shear strain was 150%. In the case of cast aluminum (marked “nontextured”), two medium and one short specimen were tested. It is seen that the development of the axial and hoop strains was delayed as compared to the curves of extruded aluminum. In all curves, no noticeable differences can be observed between specimens for shear strain of 150%, the ratio is over 0.9. For the cast specimens, the ratio is hard to determine at shear strain of 0

when f = k 2 and df = 0 (plastic state)

(6.36)

Expression (6.36a) describes the condition when the stress point is either inside the yield surface or is on the yield surface but is about to move inward; (6.36b) describes the condition when the stress point is moving on the yield surface; and (6.36c) describes the condition when the stress point is stationary on the yield surface. We make the following remarks for this model: 1. The increments of plastic strain depend on the current values of deviatoric stress and not on the stress increment. 2. The principal axes of stress and of plastic-strain-increment tensor coincide. The ﬂow rule satisﬁes the experimental ﬁnding that the plastic-strain-increment vector is normal to the yield surface if the Mises yield criterion is used. 3. No plastic volume change during plastic deformation is assumed, p that is, dεii = dλσii = 0. 4. The magnitude of plastic strain increment is determined by dλ, which in turn is determined by the actual increment of plastic work given by p

dW p = σij dεij = dλσij σij = dλ( 13 σkk δij + σij )σij = dλ( 13 σkk σii + σij σij ) = −2 dλ J2 = 2 dλ k 2

(6.37)

From (6.37), we obtain p

dλ =

σij dεij 2k 2

© 2005 by Chapman & Hall/CRC Press

p

=

((1/3)σkk δij + σij )dεij 2k 2

p

=

σij dεij 2k 2

p

=

σij deij 2k 2

(6.38)

278

Continuum Mechanics and Plasticity p

p

p

p

where dεij = 13 δij dεkk + deij = deij . A slightly different form of (6.38) can be found if we consider the following expressions: σij deij

=

σij (deije

p + deij ),

deije

=

dσij 2µ

,

dJ2 = −σij dσij = 0 (−J2 = k 2 = const) and σij deij =

σij dσij 2µ

p

(6.39) p

+ σij deij = σij deij

Using the last expression of (6.39), (6.38) becomes dλ =

σij deij 2k 2

=

σij (dεij − 13 δij dεkk ) 2k 2

=

σij dεij 2k 2

(6.40)

The Prandtl–Reuss equation may then be written as dεij =

dε σij σkm km 1 1 dσkk δij + dσij + 9K 2µ 2k 2

(6.41)

This equation relates dεij to dσij and σij , and it can be written in the form [dεij ] = [Aijkm ][dσkm ]

(6.42)

where Aijkm is a function of σij . Note that this method of determination of dλ works when f is a function of stress only and is in the form of the Mises yield criterion. In the more general expressions for f , dλ may be determined by use of the consistency condition to be discussed later. The class of perfectly plastic material is an idealization with the purpose of keeping the constitutive equation simple. This idealization is reasonable for materials that do not show signiﬁcant strain-hardening. The adequacy of this idealization depends on the purpose and requirement of the speciﬁc application. If only monotonic loading is of interest and it does not call for a reﬁned solution, then this idealization may very well lead to a satisfactory solution with a minimum amount of mathematics. However, due to the progress in industries, which give rise to problems that are subjected to complex loading conditions and impose stricter requirements, this idealization is no longer adequate in many applications. In those cases, reﬁnement of the theory is called for and strain-hardening should be considered. The reﬁnement of the ﬂow theory is discussed in Chapter 7. An example to demonstrate the differences between an elastic material and an elastic-perfectly plastic material is given by a strain-controlled test with proportional strain path as shown in Figure 6.9. Assuming that the experiment begins at point O (Figure 6.9(a)), moves to B , and continues © 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

279

(a)

(b)

C⬘

C B

B⬘ D

O⬘

O

FIGURE 6.9 (a) A proportional strain path and (b) corresponding stress trajectories for elastic (OBC) and elastic-perfectly plastic material (OBD). ,

n B⬘ B(, )

Φ

,

O

FIGURE 6.10 A controlled linear stress path and its corresponding strain path.

on to point C in the strain space. The corresponding trajectories in the stress space shown in Figure 6.9(b) are OBC for elastic material and OBD for elasticperfectly plastic material. It is seen that the two stress paths show drastic differences for the same strain path. It is a nonlinear path for the latter case. Details related to stress- and strain-controlled tests for an elastic-perfectly plastic material are discussed in Examples 6.1 to 6.3. In a stress-controlled combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, if the stress-path OB (Figure 6.10) is linear, ﬁnd the corresponding strain path.

EXAMPLE 6.1

Solution The states of stress and strain are 2 3σ σ τ 0 σij = τ σij = τ 0 0 , 0 0 0 0

τ σ − 3 0

0 0 , σ − 3

ε γ εij = 2 0

γ 2 0 0

0 0 0 (a)

© 2005 by Chapman & Hall/CRC Press

280

Continuum Mechanics and Plasticity

(b)

B

(a)

C C⬘

Φ

B⬘

O⬘

O

FIGURE 6.11 (a) A controlled proportional strain path and (b) the corresponding stress path.

Lateral strains have been neglected due to the smallness of their magnitudes, but they may be considered for better accuracy. In the elastic state from O to B (and also O B in the strain space), the relations are εe =

σ , E

γe =

τ µ

(b)

and the slope of the strain path (Figure 6.11(a)) is deﬁned by tan φ =

µσ µ εe = = tan e γ Eτ E

(c)

where is known. The strain path during the elastic state is denoted by OB’. In the elastic–plastic state, dλ = 0, and the Prandtl–Reuss equation is from (6.41) dεij =

dε σij σkm km 1 1 dσkk δij + dσij + 2 9K 2µ 2k

(d)

Since the test is stress-controlled and follows a straight path, the stress point will remain at B after yielding has occurred. Thus, dσij = 0. Hence, we have dεij =

dε σij σkm km

(e)

2k 2

The nonzero components of (e) are dε =

σ 3k 2

2 σ dε + τ dγ 3

© 2005 by Chapman & Hall/CRC Press

,

dε12 =

τ 3k 2

2 σ dε + τ dγ 3

(f)

The Flow Theory of Plasticity

281

and the strain increment has the following slope after yielding has occurred dε12 3τ = dε 2σ

dγ 3τ = dε σ

or

(g)

We now show that this direction is parallel to the normal to the yield surface at B. This is the direction of the strain path after yielding has occurred at B . The yield surface is f = 12 σij σij − k 2 = 0

(h)

For the stress state of (a), (h) reduces to f = σ 2 + 3τ 2 − 3k 2 = 0

(i)

The gradient of the yield surface is ∂f ∂f ∂σrs ∂f = = ∂σij ∂σrs ∂σij ∂σrs

1 δri δsj − δrs δij 3

=

σrs

1 δri δsj − δrs δij 3

= σij (j)

So, the components of the normal n are proportional to nσ ∝ σ11 = 23 σ ,

nτ ∝ σ12 =τ

(k)

with a slope nτ 3τ = nσ 2σ

(l)

Note that this slope is the same as that of dε12 /dε in (g). It is wrong to differentiate the yield function (i) in the τ –σ subspace to obtain the normal as nσ ∝

∂f = 2σ , ∂σ

nτ ∝

∂f = 6τ , ∂τ

nτ 3τ = nσ σ

(m)

This slope is different from that in (l). The correct way is to make distinction between σ12 and σ21 and differentiate the yield function with respect to σ12 . But, the τ –σ stress space is convenient for engineering application and, in this case, we must work with the engineering shear strain γ instead of the tensorial shear strain ε12 . Therefore, we use the γ –ε strain space, and observe that the slope in this strain space given by the second equation of (g) is the same as the slope in (m).

© 2005 by Chapman & Hall/CRC Press

282

Continuum Mechanics and Plasticity

In a strain-controlled, combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, if the strain-path OB C is linear (Figure 6.11(a)), ﬁnd the corresponding stress path.

EXAMPLE 6.2

Solution The states of stress and strain are given in (a) of Example 6.1 and the elastic phase of the problem is the same as in Example 6.1. In this range, the slope of the strain path is known and is given by m = tan φ =

ε dε µσ = = γ dγ Eτ

(a)

Yielding can occur when the stress reaches B and the strain reaches B . The last relation of (a) is σ−

mE τ =0 µ

(b)

The stresses at B may be determined from the intersection of (b) with the yield locus (6.11). They are σB =

√ 3 mkE 3µ2 + m2 E2

and

τB =

√ 3 kµ 3µ2 + m2 E2

(c)

If yielding would occur at B with a stationary stress point (Figure 6.11(b)), that is, dσij = 0, then using (6.41), the Prandtl–Reuss equation would have components dε = dε p =

σ 3k 2

2 σ dε + τ dγ , 3

dγ = dγ p =

τ k2

2 σ dε + τ dγ (d) 3

and the direction of the plastic strain increment evaluated at B would be dγ 3τB 3µ 1 = =

= dε σB mE m

(e)

We see that the slope of the strain increment in (e) is not the same as the controlled slope 1/m, and, therefore, the stress point cannot be stationary at B, and dλ = 0 at B. The stress point must move away from B in a neutral loading along the yield locus until it reaches point C, where the normal of the yield locus is parallel to the controlled strain slope O B C of Figure 6.11(a). The Prandtl–Reuss equation applies and we set the slope in (e) to 1/m, that is, σ − 3mτ = 0

© 2005 by Chapman & Hall/CRC Press

(f)

The Flow Theory of Plasticity

283

(b)

B, C

(a)

C⬘ B⬘

D⬘ at ∞

O⬘

O

D

FIGURE 6.12 (a) A controlled strain path and (b) the corresponding stress path.

The intersection between this line and the yield locus (6.11) is found at σC =

3 mk 1 + 3m2

τC =

,

k 1 + 3m2

,

with

σC = 3m = 3 tan φ τC

(g)

Thus, the slope of OC is deﬁned by angle θ as θ = tan−1 (3 tan φ)

(h)

The stress point stays at C upon further increase of the strain point beyond C . EXAMPLE 6.3 In a strain-controlled, combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, determine the stress-path that corresponds to the strain-path OB C D shown in Figure 6.12(a). Yielding occurs at B .

Solution The elastic state is governed by Hooke’s law. Plastic deformation occurs from B to C , while the stress stays at B. The states of stress and strain during this stage are

0 σij = τ 0

τ 0 0

0 0 , 0

0 σij = τ 0

τ 0 0

0 0 , 0

0

εij = γ 2 0

0

0 0

0

0

γ 2

(a)

The nonzero component of the Prandtl–Reuss equation is dγ =

© 2005 by Chapman & Hall/CRC Press

dτ τ 2 dγ + 2 µ k

(b)

284

Continuum Mechanics and Plasticity

or

τ2 dτ = µ 1 − 2 k

dγ

(c)

But, on the yield locus, using (6.11) and (a), τ 2 = k 2 . Thus, dτ = 0 and C stays at B on the yield locus. Next, we consider the stage from C to D . The strain-path C D has increment in the axial strain only, while the shear strain is kept constant, that is, dγ = 0. Due to the effect of elastic strain, dγ p = 0. Therefore, plastic deformation occurs. The states of stress and strain are the same as that of (a) of Example 6.1. Putting dγ = 0, the shear component of the Prandtl–Reuss equation (6.41) is dτ = −

2σ τ µ dε + 3τ 2

(d)

σ2

Substituting (d) into the differential form of yield function (6.11), we obtain dσ =

6τ 2 µ dε σ 2 + 3τ 2

(e)

It is easy to show that the stress increment (dτ , dσ ) is tangential to the yield locus. This is not a neutral loading, however, because the plastic strain is taking place. The plastic strain increments are found from (6.41) as dεp =

2 σ 2 dε 9 k2

and

dγ p =

2 σ τ dε 3 k2

with dγ = 0

(f)

By use of (d) and (e), both dτ and dσ may be calculated for a given dε. These equations may be integrated to obtain a closed form solution. From (d) and (6.11), we have 2µτ k 2 − τ 2 dτ = − dε √ 3 k2

or

τ

dτ k2

− τ2

2µdε = −√ 3 k2

(g)

This equation may be integrated to obtain √ 3k 1 − 1 − (τ/k)2 ε= ln 2 µ τ/k

(h)

where, by use of the boundary condition that τ = k when ε = 0, the integration constant is zero. Introducing now nondimensional variables X = µε/k

© 2005 by Chapman & Hall/CRC Press

Nondimensional Stresses

The Flow Theory of Plasticity 1

285

Z

0.8 0.6 0.4 Y 0.2 0

2 4 6 8 Nondimensional Axial Strain, X

10

FIGURE 6.13 Nondimensional shear (Y) and axial (Z) stresses as axial strain increases.

for strain and Y = τ/k for stress, (h) may be solved for Y to yield Y=

√ 3 √ 1 + e(4X)/ 3

2e(2X)/

(i)

Figure 6.13 shows the plot of Y versus X. It is seen that the shear stress gradually reduces as the axial strain increases. Similarly, (e) may be integrated to yield √

σ −1 + e(4X)/ 3 √ Z= √ = 3k 1 + e(4X)/ 3

(j)

Z may be plotted against X and the relationship is also shown in Figure 6.13. Using (i) and (j), X may be eliminated to obtain Y 2 + Z2 = 1

(k)

which is the yield locus (6.11). Thus, the stress point moves, generating plastic deformation, along the yield locus and end up in D as shown in Figure 6.12(b). √ Deﬁne an equivalent (effective) stress as σ¯ = 3/2{σij σij }1/2 √ and an equivalent (effective) plastic strain increment as d¯ε p = 2/3× p p p {dεij dεij }1/2 , show that the plastic work increment is dW p = σij dεij = σ¯ d¯ε p . EXAMPLE 6.4

Solution From (6.37), we have p

dW p = σij dεij = 2dλ k 2

© 2005 by Chapman & Hall/CRC Press

(a)

286

Continuum Mechanics and Plasticity

Using (6.32), (6.34), and (a), the equivalent plastic strain increment is

2 p p 1/2 dεij dεij = d¯ε = 3 2 dλ 2 dW p =√ k = √ 3 k 3k

p

2 1/2 dλ σij σij = 3

√ 2 dλ( 2k) 3 (b)

Thus, dW p =

√ 3k d¯εp

(c)

On the other hand, the equivalent stress is σ¯ =

3 1/2 = σ σ 2 ij ij

√ 3 √ ( 2k) = 3k 2

(d)

Combining (c) and (d), we obtain p

dW p = σij dεij = σ¯ d¯εp

(e)

Note that equivalent (or effective) quantities such as the equivalent (or effective) stress, the equivalent (or effective) strain, or the equivalent (or effective) strain rate are often used in dealing with the multidimensional behavior of isotropic materials. This equivalent quantity often represents the magnitude of that quantity.

6.5

Strain-Hardening

There are three classes of materials: the strain-hardening material, the perfectlyplastic material, and the strain-softening material. Generally, metals are strainhardening (or work-hardening) materials and geotechnical materials may exhibit strain-softening under certain conditions. Several criteria have been proposed to classify the materials. Generally, the strain-hardening material is regarded as a stable material. Drucker [21] proposed to classify materials by the now well-known Drucker’s postulate, which is not a law of thermodynamics, but a means of classiﬁcation. Materials obeying Drucker’s postulate can then be studied by a theory of plasticity that can be built up based on that postulate. In the multiaxial stress state, strain-hardening is considered in the form of hardening rules for subsequent yield surfaces. Experimental determination of subsequent yield surfaces is discussed in Chapter 7. It has been observed that the yield surface, upon application of a deformation history, will undergo expansion, distortion, translation, and rotation. A precise description of these

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

287

characteristics is deferred to Chapter 12. In this section, we discuss a simpliﬁed version of the hardening rules and consider only the expansion (isotropic hardening) and translation (kinematic hardening) of the yield surface. This simpliﬁed version has been widely used in the mechanics literature. 6.5.1

Drucker’s Postulate

Drucker’s postulate consists of two parts: the stability in the small and the stability in the large. These are described by the following statements: 1. The stability in the small: The work done by an external agency, which slowly applies an additional set of forces to the already stressed material, over the displacement it produces, is positive. 2. The stability in the large: The net work performed by the external agency over the cycle of application and removal is positive, if plastic deformation has occurred in the cycle. The aforementioned external agency is entirely separate and distinct from the agency that causes the existing state of stress and that has produced the existing state of strain. The cycle of application is the stress cycle and is different from Ilyushin’s strain cycle, which is not as restrictive as the stress cycle. The meaning of the above statements are now explained. In the one-dimensional case, let us consider Figure 6.14(a). The stress at A is already the existed state. The stability in the small says that an external agency increases the stress from A to C and the work done represented by area ACE is positive; the stability in the large says that the work done by the external agency over the stress cycle of σ ∗ to σA and then to σC and then back down to σ ∗ and represented by area BACDB is positive. σ ∗ is an arbitrary stress state in the elastic region. In the multidimensional case, we consider a stress cycle described in Figure 6.14(b). At time t = 0, the stress point is at B and denoted by σij∗ , which is an arbitrary point within or on the current yield surface, so that p

f (σij∗ , εij , κ) ≤ 0 (a)

*

A

(b)

C E

t1, ij

B t = 0, ij* tf, D

B D

FIGURE 6.14 Stress cycles: (a) one-dimensional and (b) multiaxial.

© 2005 by Chapman & Hall/CRC Press

A

(6.43)

C + d , t ij ij 2

p

p

f (ij +dij, ij +dij , + d ) = 0 p

f (ij, ij , ) = 0

288

Continuum Mechanics and Plasticity

where κ is a strain-hardening parameter. The yield function is expressed in terms of stress σij , which is possible as in (6.12) or (6.13). Furthermore, for strain-hardening materials, the yield function f depends on the prestraining p history and we include the plastic strain εij and a parameter κ in the yield function for generality. At point A (t = t1 ), the stress point σij is on the yield surface so that p

f (σij∗ , εij , κ) = 0

(6.44)

The stress point then pierces the yield surface and carries the yield surface with it, until at point C, where t2 = t1 +dt, it reaches the dashed curve which is governed by p

p

f (σij + dσij , εij + dεij , κ + dκ) = 0

(6.45)

Additional plastic deformation has occurred during this step. Unloading then follows, which brings the stress point back to σij∗ at B. The corresponding time is t = tf . At this point, p

p

f (σij∗ , εij + dεij , κ + dκ) ≤ 0

(6.46)

The work done during this stress cycle is W=

0

tf

(σij − σij∗ )˙εij dt =

t2

t1

p

(σij − σij∗ )˙εij dt ≥ 0

(6.47)

The last expression has accounted for the fact that the work done by the elastic strain dεije for a closed path is zero. In this stress cycle, the plastic deformation only occurs in the step AC. We now take Taylor series expansion of the above integral about t = t1 as p p p W (t2 ) = (σij − σij∗ )˙εij t=t dt + 12 [σ˙ ij ε˙ ij + (σij − σij∗ )¨εij ]t1 (dt)2 + · · · ≥ 0 1

(6.48) with W (t1 ) = 0. For the stability in the small, σij∗ and σij coincide at t1 , and the above expression is reduced to p

W = 12 σ˙ ij ε˙ ij (dt)2 + · · · ≥ 0

(6.49)

Take the time increment dt small enough that the higher order terms in dt are negligible, we obtain p

σ˙ ij ε˙ ij ≥ 0

or

p

dσij dεij ≥ 0

which is the expression for the stability in the small.

© 2005 by Chapman & Hall/CRC Press

(6.50)

The Flow Theory of Plasticity

289

In the case of σij∗ = σij at t1 , by neglecting the second and higher order terms, we have from (6.48) p

W = (σij − σij∗ ) ε˙ ij dt ≥ 0

p

(σij − σij∗ ) dεij ≥ 0

or

(6.51)

This is the expression for the stability in the large. By the use of Drucker’s postulate, it is possible to show that the yield surface is convex and that the plastic strain increment is normal to the yield surface. Without the use of this postulate, these two effects would have been two separate assumptions. We discuss the case that the yield surface is smooth without corners. Let σij be any regular point on the yield surface and σij∗ p be an arbitrary point inside or on the yield surface. Let dεij be the plastic p strain increment at σij . Then, (6.51) shows that the vectors (σij − σij∗ ) and dεij are making an acute angle and that the arbitrary σij∗ must lie on the side p

p

of the hyperplane opposite to that from which dεij is directed. dεij is normal to the hyperplane as shown in Figure 6.15(a). Since σij is a regular point of the yield surface, the hyperplane must be tangent to the yield surface, and, p therefore, dεij is normal to the yield surface at the point of tangency σij . This also establishes the convexity of the yield surface at point σij . p Next, we show that the direction of dεij is independent of the direction of (σij − σij∗ ) if the yield surface is regular. Assuming that two different (σij − σij∗ ) p give rise to two different dεij . Then, the yield surface f1 = 0, which is perp(1) pendicular to dεij must intersect with the yield surface f2 = 0, which is p(2) perpendicular to dεij at an angle (see Figure 6.15(b)). Thus, the yield surface is nonregular at σij , which contradicts with the assumption that it be p regular at σij . Therefore, the two dεij ’s must not be different and the direction p of dεij is independent of the direction of (σij − σij∗ ). In the case when f = 0 is nonregular at σij , the normality condition cannot be p established. Drucker’s postulate only requires that dεij lie within a bounded angle at a pointed vertex of the yield surface. However, nonregular yield

(a)

(b)

p

dij

p(1)

dij

p(2)

dij

Hyperplane p normal to dij ij ij*

FIGURE 6.15 Normality of plastic strain increment.

© 2005 by Chapman & Hall/CRC Press

=0

f1

f2

=0

290

Continuum Mechanics and Plasticity

surfaces have not been experimentally observed as mentioned in Section 6.2. Therefore, this case will not be pursued.

6.5.2

The Isotropic-Hardening Rule

We call a strain-hardening an isotropic hardening, if the subsequent yield surface is an isotropic expansion of the initial yield surface as shown in Figure 6.16(a). The Bauschinger effect is not considered in the isotropic hardening. The yield function is expressed by f (σij ) = Y 2

(6.52)

where Y is the yield stress under uniaxial tension. Y represents the radius of the yield surface and, when it increases, the yield surface expands in size. Y can be a function of either one of the two quantities that are used to measure the degree of hardening: the plastic work per unit volume deﬁned by Wp =

p

σij dεij

(6.53)

or the equivalent plastic strain with increment deﬁned by p

d¯ε =

2 p p 1/2 dεij dεij 3

(6.54)

An equivalent stress deﬁned by σ¯ =

(a)

3 1/2 σ σ 2 ij ij

(6.55)

(b)

ur

fa c

e

q Su bse

t uen

rfa

ce

S

Su

I n i t i a l Yi el d

l Yie

d

FIGURE 6.16 (a) Isotropic hardening and (b) schematic equivalent stress–plastic strain curve.

© 2005 by Chapman & Hall/CRC Press

p

The Flow Theory of Plasticity

291

is usually introduced to describe the isotropic hardening. The equivalent stress can also take the following forms σ¯ = =

1 2 2 2 1/2 (σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 + 6σ12 + 6σ23 + 6σ31 2 1/2 1 (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 2

(6.56)

The equivalent√stress is deﬁned based on the Mises yield criterion (6.6), √ observing Y = 3 k. Equation (6.6) reduces to Y = (3/2){σij σij }1/2 , which is of the same form as (6.55). Thus, σ¯ = Y and we write either Y = σ¯ = F(W p )

(6.57)

or

d¯εp

Y = σ¯ = H

(6.58)

where F and H are functions and these functions are to be determined by plotting experimental stress–strain curves in the form of σ¯ versus ε¯ p as shown in Figure 6.16(b). There are efforts to obtain a universal stress–strain curve, such as (6.57) or (6.58), which encompasses all states of stress [22]. Using this concept, a shear stress–strain curve can be deduced from a tensile stress–strain curve. We invert the function of (6.58) to obtain

d¯εp = H −1 (σ¯ ) or

ˆ σ¯ )dσ¯ d¯ε p = F(

(6.59)

where the function H is known from experiment. Using the ﬂow rule (6.35), the equivalent plastic strain increment is from (6.54) p

d¯ε =

2 2 1/2 = dλ σij σij 3

2 2 2 dλ σ¯ = dλσ¯ 3 3 3

(6.60)

Equating (6.59) and (6.60), we ﬁnd dλ =

3 F(σ¯ )dσ¯ 2

where F(σ¯ ) =

ˆ σ¯ ) F( σ¯

(6.61)

Therefore, the ﬂow rule is written as p

dεij = 32 F(σ¯ )dσ¯ σij

© 2005 by Chapman & Hall/CRC Press

(6.62)

292

Continuum Mechanics and Plasticity

In the case of uniaxial tension, (6.62) reduces to p

dε p = dε11 = 32 F(σ¯ )dσ¯ ( 23 σ ) = F(σ¯ )dσ¯ σ

(6.63)

and, in the case of pure torsion in a thin tube, (6.62) is p 1 2 dγ

p

= dε12 = 32 F(σ¯ )dσ¯ τ

(6.64)

The expression of equivalent stress for uniaxial tension is σ¯ =

3 1/2 {σ σ } = 2 ij ij

2 σ 2 1/2 3 2 =σ σ +2 − 2 3 3

(6.65)

and for pure torsion is σ¯ =

3 1/2 = σ σ 2 ij ij

√ 3 {2τ 2 }1/2 = 3 τ 2

(6.66)

Thus, we ﬁnd σ τ=√ 3

(6.67)

Substituting (6.67) into (6.63) and (6.64), we obtain dγ p =

√ 3 dεp

(6.68)

We now use (6.67) and (6.68) to deduce a shear stress–strain curve (τ , γ ) from a known tensile stress–strain curve (σ , ε). In a monotonic loading condition, (6.68) is integrated to yield γp =

√ p 3ε

or

(γ − γ e ) =

√ 3(ε − ε e )

or

γ−

√ τ σ = 3 ε− µ E (6.69)

Using (6.67) and the relations of elastic constants, (6.69) reduces to γ √ =ε− 3

1 − 2ν 3E

σ

(6.70)

where ν is Poisson’s ratio. Knowing (σ , ε) for any point on the tensile curve, we can use (6.67) and (6.70) to determine the corresponding point (τ , γ ) on the shear curve. We can also use a graphical method to accomplish the task. Referring to Figure 6.17, we need to establish ﬁrst, the two elastic lines with slopes E and µ. At point A on the tensile line, the stress is σA . Segment AB is the

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

293

corresponding plastic strain ε p , which is known. Next, locate point C on the √ elastic shear line with stress equals to σ / 3. The length of line segment CD A √ is 3 εp and, therefore, point D can be located. The process may be repeated for all points to determine the shear stress–strain curve. In the case of combined axial–torsion of a thin-walled tube, if we use the Mises yield function and isotropic hardening, the ﬂow rule is given by (6.62). (a) Determine the function F(σ¯ ) from a uniaxial tension test. (b) For the general case of combined tension and torsion, ﬁnd the expressions for the axial and shear strain increments. (c) For a stress-controlled proportional stress-path OBC shown in Figure 6.18, ﬁnd the corresponding strain path. (d) For a stress-controlled torsion from O to Afollowed by tension ABCD while

EXAMPLE 6.5

le Tensi

A

B(, )

A C A

Shear

D(, )

E

3

AB = p CD = 3 p

FIGURE 6.17 Determination of shear stress–strain curve from the tension stress–strain curve.

, D⬘

n B⬘

C B (, )

Φ

n

fC fB

,

O FIGURE 6.18 Stress-controlled proportional stress path assuming isotropic hardening.

© 2005 by Chapman & Hall/CRC Press

294

Continuum Mechanics and Plasticity dp

B

A

C

O

D

FIGURE 6.19 A torsion–tension stress path assuming isotropic hardening.

keeping the shear stress constant at τA (Figure 6.19), discuss the corresponding strain path. Solution For a combined axial–torsion test, the states of stress and strain are 2 γ σ τ 0 3 0 ε σ τ 0 γ 2 σ σij = τ 0 0 , σij = τ εij = − 0 , 0 0 3 2 0 0 0 σ 0 0 0 0 0 − 3 (a) The equivalent stress and its increment are from (6.55) and (a) σ¯ = {σ 2 + 3τ 2 }1/2 ,

dσ¯ =

σ dσ + 3τ dτ σ¯

In the case of uniaxial tension, the Prandtl–Reuss equation is dσ 3 2 dε = dε11 = + F(σ¯ )dσ¯ σ E 2 3

(b)

(c)

and the equivalent stress and its increment are σ¯ = σ ,

dσ¯ =

σ dσ σ¯

(d)

Using (d), (c) may be written as dε 1 F(σ¯ )σ 2 1 = = + dσ Et E σ¯

© 2005 by Chapman & Hall/CRC Press

(e)

The Flow Theory of Plasticity

295

where Et is the slope of the tensile stress–strain curve. Solving (e), we ﬁnd F(σ¯ ) =

1 σ¯

1 1 − Et E

(f)

For the general case of combined tension and torsion, by use of the ﬂow rule (6.62) and the elastic strains, the two components of the Prandtl–Reuss equation are

1 1 − (σ dσ + 3τ dτ ) Et E dτ 1 3τ 1 dγ = + (σ dσ + 3τ dτ ) − µ E (σ¯ )2 Et σ dσ + dε = E (σ¯ )2

(g)

For the stress-controlled proportional stress-path OBC shown in Figure 6.18, the elastic state OB is the same as that of Example 6.1 and shown previously in Figure 6.10 with angle φ. At point B of Figure 6.18, yielding ﬁrst occurs with corresponding yield locus fB . The normal to the yield locus is denoted by n. As the stress path proceeds from B to C, the stress point carries the yield locus with it and the yield locus makes an isotropic expansion. The normal to the yield locus fC at C is still n. Taking the plastic strain part of (g), we obtain the following ratio for the plastic strain increments 3τ dγ p = p dε σ

(h)

It is easily shown that this slope is normal to the yield locus. However, the strain-path B D is not in the same direction as the normal n because of the elastic strain. Path B D has to be determined by integrating (g). We now discuss a stress-controlled torsion from O to A followed by tension ABCD while keeping the shear stress constant at τA (Figure 6.19). During the stage of tensile loading ABCD, the strain increments are given by (g) with dτ = 0. Thus, dσ 1 1 σ2 dε = − + (dσ ) E E (σ¯ )2 Et 3τA σ 1 1 dγ = − (dσ ) E (σ¯ )2 Et

(i)

We see from (i) that the plastic strain ratio is 3τA dγ p = = tan ϕ p dε σ

(j)

The angle ϕ of the plastic strain vector changes from 90◦ at A to smaller angles as the axial stress σ increases. As σ becomes large, the angle ϕ tends

© 2005 by Chapman & Hall/CRC Press

296

Continuum Mechanics and Plasticity

to zero. We note that this result is merely a prediction of the model with isotropic hardening. Related experimental results are discussed in Chapter 7. The plastic-strain-increment vectors are shown in Figure 6.19. Finally, we mention that the strain path is found by integrating the expression (k) which is obtained by eliminating dσ from (i) dγ [3τA σ/(σ¯ )2 ][(1/Et ) − (1/E)] = dε 1/E + (σ 2 /(σ¯ )2 )[(1/Et ) − (1/E)]

6.5.3

(k)

The Kinematic-Hardening Rule

The kinematic-hardening rule assumes that the yield surface translates without rotation in the stress space. The shape and size of yield surface remain unchanged during motion of yield surface. This hardening rule has been introduced by Prager [23] to account for Bauschinger effect. Hodge [24] pointed out that the concept of kinematic hardening must be applied in the nine-dimensional stress space. In the nine-dimensional space, the initial yield surface is given by f (σij ) = 0

(6.71)

and the subsequent yield surface by f (σij − αij ) = 0

(6.72)

where αij is the total translation of center of initial yield surface and is termed back stress by some investigators. Note that for Mises criterion, we write

σij − αijD σij − αijD = 2k 2

(6.73)

where αijD is the deviatoric part of αij . Hodge [24] further suggested the concept of combined isotropic–kinematic hardening. In this case, the yield surface translates, deﬁned by αij , and expands as well, which is deﬁned by the change in k. The evolution rule of αij in the stress space is of interest. Prager [23] proposed a linear-hardening rule as p

dαij = c dεij

(6.74)

where c is a constant. Ziegler [25] proposed a modiﬁed kinematic-hardening rule as dαij = dµ(σij − αij )

© 2005 by Chapman & Hall/CRC Press

where dµ > 0

(6.75)

The Flow Theory of Plasticity

297

The directions of dαij are different between (6.74) and (6.75) and they are shown in Figure 6.20. In (6.75), dµ is a parameter and should not be mixed with the shear modulus. In the ﬁgure, O is the origin of the nine-dimensional stress space and O is the center of the current yield surface. The current stress point is at P. According to (6.74), the center of yield surface would translate in a direction normal to the yield surface at P and this increment of (P) translation is denoted by dαij in the ﬁgure. On the other hand, according (Z) to (6.75), the increment of translation of the yield surface, denoted by dαij , is along the direction of O P. We note that the two rules are the same if the current yield surface is a hypersphere, which is true when the Mises yield surface is considered and a combined isotropic–kinematic hardening is applied. The linear kinematic hardening can only be applied to a material with a bilinear stress–strain curve when unloading and reverse loading is considered. For a nonlinear stress–strain curve, the linear kinematic-hardening rule would result in an unloading curve, which bends in an unnatural way and such an unloading curve has never been observed. Figure 6.21(a) shows such (p)

dij

(z)

dij

O⬘

P

ij

ij f=0

O

ij

FIGURE 6.20 Kinematic-hardening rules by Prager and Ziegler.

(a)

(b) rve d cu Loa

Y

h

O

h

ss k stre Bac

cu load Un

rve

p

h

FIGURE 6.21 Linear kinematic-hardening: (a) nonlinear stress–strain curve and (b) bilinear stress–strain curve.

© 2005 by Chapman & Hall/CRC Press

298

Continuum Mechanics and Plasticity

a behavior in the one-dimensional loading–unloading stress–strain curve. The linear kinematic hardening rule, applied to a bilinear stress–strain curve (a special case of (6.58)), is shown in Figure 6.21(b), where the stress σ is plotted against the plastic strain ε p . In the ﬁgure, Y is the initial yield stress and the slope of the linear kinematic hardening is h, that is, dα = h dεp

(6.76)

In the case of uniaxial loading, the increment of the back stress is

dα dαij = 0 0

0 0 0

0 0 0

and

2 3 dα dαijD = 0 0

0 −

dα 3 0

−

0 0 dα

(6.77)

3

Thus, from (6.74), the ﬁrst element of the linear kinematic hardening rule is 2 3 dα

= c dεp

(6.78)

Comparing (6.76) with (6.78), we obtain h = 32 c

(6.79)

and the stress–stress curve during loading is given by σ = Y + h εp

(6.80)

Thus, h is also the slope of the stress–strain curve. In case of nonlinear loading curve, the yield function is f (σij − αij ) = Y 2

(6.81)

in which both Y and αij are not constant for combined isotropic–kinematic hardening. The increment of stress in the uniaxial stress σ versus plastic strain ε p plot consists of two parts, that is, dσ = dY + dα

(6.82)

Introduce an isotropic–kinematic-hardening parameter β, which is a number 0 ≤ β ≤ 1. Then, we may write dY = βh dεp

© 2005 by Chapman & Hall/CRC Press

and

dα = (1 − β)h dε p

(6.83)

The Flow Theory of Plasticity

299

and (6.82) becomes dσ = h dε p

(6.84)

The extreme value β = 1 characterizes isotropic hardening and β = 1 characterizes kinematic hardening. When β has a value between 0 and 1, then we have a case of combined isotropic–kinematic hardening. The combined isotropic-linear kinematic-hardening rule cannot lead to a reasonable unloading curve. Nonlinear kinematic-hardening rules will have to be used to describe the unloading curve. A nonlinear kinematic-hardening rule was ﬁrst used by Armstrong and Frederick [26] and written as p

dαij = 23 c dεij − καij d¯ε p

(6.85)

where c and κ are material constants. This rule has gained popularity in recent literatures. We will see in Chapter 8 that this hardening rule is also a part of the endochronic theory of plasticity proposed by Valanis [27] and was applied by Wu and Yang [28] and Wu et al. [29]. Denoting the increment of equivalent plastic strain by the increment of a monotonically increasing positive parameter z, so that dz = |d¯ε p |

(6.86)

then (6.85) may be written as p

dαij 2c dεij + καij = dz 3 dz

(6.87)

If c and κ are constants, then (6.87) is a linear ordinary differential equation with constant coefﬁcients and the solution is 2c αij (z) = 3

p

z

e

−κ(z−z )

z0

dεij (z ) dz

dz + αij (0) e−κ(z−z0 )

(6.88)

In (6.88), z is the current value of the parameter; z0 is the initial value of z; and αij (0) is the initial value of αij (z). In the case of uniaxial loading–unloading, (6.90) reduces to α(z) =

2c 3

z

z0

e−κ(z−z )

dε p (z ) dz + α(0) e−κ(z−z0 ) dz

(6.89)

Referring to Figure 6.22, let us consider loading along OA and then unloading to B. The initial conditions are z0 = 0 and α(0) = 0. We note that

© 2005 by Chapman & Hall/CRC Press

300

Continuum Mechanics and Plasticity A

Normalized Back Stress

0.4 0.3 0.2 B

0.1

O

0.01

0.02 0.03 Strain p

0.04

0.05

FIGURE 6.22 Loading–unloading curves for nonlinear kinematic-hardening.

[dε p (z )/dz ] = +1 during loading, and [dε p (z )/dz ] = −1 during unloading. Using these conditions, (6.89) may be integrated during loading to yield y = 1 − e−κz = 1 − e−κε

p

with y =

3κ α 2c

(6.90)

where y is a normalized back stress. Unloading occurs at point A and (6.89) is integrated to obtain the unloading curve as α(z) =

2c 3

0

zA

e−κ(zA −z ) (+1) dz +

= α(zA ) +

2c 3

z

zA

2c 3

z

zA

e−κ(z−z ) (−1) dz =

e−κ(z−z ) (−1) dz + α(0)e−κ(z−z0 ) 2c 2c [1 − e−κzA ] − [1 − e−κ(z−zA ) ] 3κ 3κ

2c −κzA −κ(z−2zA ) = [e − 1] e 3κ

(6.91)

The value of z at A is denoted by zA . Referring to (6.86), during loading, we have dz = d¯εp = dεp ; but during unloading, when z > zA , we have dz = −dεp . This relation may be integrated starting from point A to obtain ε = εA + zA − z = 2zA − z

(6.92)

Substituting (6.92) into (6.91), we obtain p

y = e−κεA [eκε − 1] p

(6.93)

Equations (6.90) and (6.93) are plotted in Figure 6.22. We see that the curves for loading and unloading do not coincide and they are curved. The slopes for loading and unloading curves starting at any point such as A are different. © 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

301

The differential form (6.85) for the uniaxial loading–unloading is dα = c dε p − κα d¯ε p = (c − κα)dε p = (c + κα)dε

for loading

p

for unloading

(6.94)

where (6.94) deﬁnes the slopes for the two cases. Finally, we mention that the linear kinematic-hardening rule leads to a straight line applicable to both loading and unloading. 6.5.4

General Form of Subsequent Yield Function and its Flow Rule

In order to have a more general description of yield surface, let us consider p that the yield function is a function of stress σij , plastic strain εij , and a parameter κ, and write p

f (σij · εij , κ) = 0

or

p

f (σij · εij , κ1 ) = κ0 = const

(6.95)

where κ0 represents the size of the yield surface. Referring to Figure 6.23, p points A and B have the same εij and κ0 , and, without κ1 , we are not able p to distinguish A from B. We have to know dεij and dκ1 to determine the subsequent yield surface. The ﬂow rule is from (6.32) p

dεij = dλ

∂f ∂σij

(6.32)

On the other hand, Drucker’s postulate gives p

dσij dεij = dλ dσij

∂f >0 ∂σij

(6.96)

where (∂f /∂σij )dσij > 0 represents the loading condition. Comparing the above two expressions we found dλ > 0. A

O

B

FIGURE 6.23 Parameters for yield surface.

© 2005 by Chapman & Hall/CRC Press

302

Continuum Mechanics and Plasticity

The parameter dλ is determined by use of the consistency condition, Prager [30]. Since loading from a plastic state must again lead to a plastic state, the stress and plastic strain that exist after the inﬁnitesimal changes p dσij , dεij , and dκ have taken place must still satisfy (6.97), which is p

f (σij , εij , κ) = 0

(6.97)

By use of the consistency condition, the increment of the yield function is zero, that is, df =

∂f ∂f ∂f p + dκ = 0 dσij + p dεij + ∂σij ∂κ ∂εij (A)

In Figure 6.24, the stress at point A is σij

(6.98)

and it is on the yield surface

(A) p(A) f σij , εij , κ (A) = 0

(6.99)

An inﬁnitesimal loading has moved the stress point from A to B and it carries (B) the yield surface with it, so that the stress at B is σij and the yield surface that B is on is (B) p(B) f σij , εij , κ (B) = 0

(6.100)

(B) p(A) f σij , εij , κ (A) > 0

(6.101)

while

Substituting (6.32) into (6.98), we have df =

∂f ∂f ∂f ∂f dσij + dλ p + dκ = 0 ∂σij ∂κ ∂εij ∂σij

(B)

Β, ij

(A)

A, ij

FIGURE 6.24 The consistency condition.

© 2005 by Chapman & Hall/CRC Press

(6.102)

The Flow Theory of Plasticity

303

which may be solved to obtain dλ as dλ = −

(∂f /∂κ)dκ + (∂f /∂σij )dσij

(6.103)

p

(∂f /∂σrs )(∂f /∂εrs )

Therefore, by use of (6.32), the ﬂow rule is p

dεij =

(∂f /∂κ)(∂f /∂σij )dκ + (∂f /∂σkm )(∂f /∂σij )dσkm p

−[(∂f /∂σrs )(∂f /∂εrs ]

(6.104)

Note that this equation consists of two parts. One part is due to dκ and the other part is due to dσij ; but the stress increments appear in the scalar form involving summation. p The increment dκ may be assumed to be a linear function of dεij , such that p

p

p

p

dκ = hrs (σmn , εmn )dεrs = h11 dε11 + h12 dε12 + · · ·

(6.105)

Then, dκ = hkm dλ

∂f ∂σkm

(6.106)

By use of (6.106), (6.102) reduces to ∂f ∂f ∂f ∂f ∂f df = =0 dσij + dλ + hkm p ∂σij ∂κ ∂σkm ∂εij ∂σij

(6.107)

We then solve (6.107) for dλ to obtain dλ =

−(∂f /∂σij )dσij p

(∂f /∂σrs )(∂f /∂εrs ) + (∂f /∂κ)(∂f /∂σrs )hrs

(6.108)

Therefore, (∂f /∂σkm )(∂f /∂σij )dσkm

p

dεij =

p

−[(∂f /∂σrs )(∂f /∂εrs ) + (∂f /∂κ)(∂f /∂σrs )hrs ]

(6.109)

p

This equation shows that dεij is linearly related to dσkm and (6.109) is in the following form p

p

dεij = Aijkm (σrs , εrs , κ)dσkm

© 2005 by Chapman & Hall/CRC Press

(6.110)

304

Continuum Mechanics and Plasticity

We have thus shown that the linear relation of (6.110) between the plastic strain and stress increments follows from the normality condition of plastic strain-rate by assuming a linear relationship for dκ given by (6.105). A special case of (6.110) is, Hill [16, p. 33], p

dεij = Gij

∂f dσkm ∂σkm

(6.111)

where Gij is a symmetric function of stress and strain history, but is not a function of dσkm . In addition, Gii = 0. Equation (6.111) has been applied in [16] to the case of isotropic hardening. If we choose ∂g ∂σij

(6.112)

∂g ∂f dσkm ∂σij ∂σkm

(6.113)

Gij = h then, (6.111) becomes p

dεij = h

in which h = h( J2 , J3 ) and g = g( J2 , J3 ) is the plastic potential. We see that (6.113) is in the form of (6.109). Another special case of (6.112) is p

dεij = G

∂f ∂f dσkm ∂σij ∂σkm

(6.114)

This form was used by Drucker [31]. In the equation, G is any positive scalar function of stress, strain, and history κ, but is independent of dσkm . An important special case is the kinematic hardening. Consider the yield function f (σij − αij ) = 0

(6.115)

in the stress space. Let pij = σij − αij , then ∂f ∂pij ∂f ∂f ∂f = = δik δjm = ∂σkm ∂pij ∂σkm ∂pij ∂pkm ∂f ∂f ∂pij ∂f = =− ∂αkm ∂pij ∂αkm ∂pkm

(6.116)

Thus, ∂f ∂f =− ∂σij ∂αij

© 2005 by Chapman & Hall/CRC Press

(6.117)

The Flow Theory of Plasticity

305

Using the yield function (6.115), the consistency condition is df =

∂f ∂f dσij + dαij = 0 ∂σij ∂αij

(6.118)

Using (6.117), we then have ∂f ∂f dσij − dαij = 0 ∂σij ∂σij

(6.119)

If we apply Prager’s linear-hardening rule, we obtain ∂f ∂f p dσij − c dεij = 0 ∂σij ∂σij

(6.120)

∂f ∂f ∂f dσij − c dλ =0 ∂σij ∂σij ∂σij

(6.121)

or

Hence, (∂f /∂σkm )dσkm c[(∂f /∂σij )(∂f /∂σij )]

(6.122)

(∂f /∂σij )(∂f /∂σkm )dσkm c[(∂f /∂σij )(∂f /∂σij )]

(6.123)

dλ = and the ﬂow rule is p

dεij =

This equation may also be derived from (6.106) by setting dκ = 0. Equation (6.104) becomes p

dεij =

(∂f /∂σij )(∂f /∂σkm )dσkm p

−[(∂f /∂σrs )(∂f /∂εrs )] p

(6.124) p

In this case, the yield function is given by f (σij , εij ) = 0, where σij and εij are treated as independent variables. By use of Prager’s linear-hardening rule, we write ∂f p ∂εrs

=

∂f ∂f c=− c ∂αrs ∂σrs

(6.125)

Combining (6.124) and (6.125), we obtain (6.123). If we use Ziegler’s kinematic-hardening rule, then dαij = dµ(σij − αij )

© 2005 by Chapman & Hall/CRC Press

with dµ > 0

(6.126)

306

Continuum Mechanics and Plasticity

The consistency condition is ∂f ∂f dσij − dµ (σij − αij ) = 0 ∂σij ∂σij

(6.127)

dµ =

(∂f /∂σij )dσij (σkm − αkm )(∂f /∂σkm )

(6.128)

dαij =

(∂f /∂σrs )dσrs (σij − αij ) (σkm − αkm )(∂f /∂σkm )

(6.129)

df = Therefore, we obtain

and

p

We see that the evolution of αij is not directly related to dεij . But, the ﬂow rule for this case is still given by (6.32), in which dλ cannot be determined from the consistency condition. Instead, dλ is determined from the normality condition as follows: we deﬁne a plastic modulus K along the direction of the outward normal n at the stress point on the yield surface. The stress increment projected along n is dσ = n · dσ and the following relation holds: (n · dσ)n = K dεp

with K > 0

(6.130)

Therefore, the ﬂow rule is dεp =

6.6

1 dσ (n · dσ)n = n K K

(6.131)

The Return-Mapping Algorithm

We discussed in Section 6.5.4 how the plasticity factor dλ can be determined by means of the consistency condition of Prager [30]. This method has been applied extensively in the literature to solve boundary-valued problems of plastic deformation involving simple states of stress. For multidimensional engineering problems of plasticity, a numerical algorithm has been developed, which is known as the return-mapping algorithm (or the backward Euler integration algorithm). For constitutive equations in the rate form, the numerical procedure calls for the determination of quantities at step (n + 1) using information at step (n). The return-mapping algorithm assures that the incremental step from (n) to (n + 1) is consistent with the ﬂow rule and hardening rule, and the stress point at step (n + 1) is lying on the subsequent yield surface. Referring to Figure 6.25, the current stress σ (n) is at A and the stress at the next step σ (n+1) is at B. The task is to determine the stress at point B

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

307 C, T(n + 1) F

A, (n)

E

B, (n + 1) D ∆e

∆ p ∆ E

FIGURE 6.25 The return-mapping algorithm in one-dimensional stress.

for a strain increment ε. Starting from A, point C is the trial step known as the elastic predictor, its stress denoted by σ T(n+1) . DC is obtained by multiplying the total strain increment ε by the elastic modulus E. From the ﬁgure, we see that AE is the plastic strain increment ε p and ED is the elastic strain increment εe . BC is equal to EF, which is obtained by multiplying εp by the elastic modulus E. BC is known as the plastic corrector. The stress increment DB = elastic predictor − plastic corrector = DC − BC. In the multidimensional case, the algorithm is formulated below: The elastic predictor is T(n+1)

σij

(n)

(n+1)

= σij + Cijkm εkm p(n+1)

and the plastic corrector is Cijkm εkm (n+1)

σij

T(n+1)

= σij

p(n+1)

− Cijkm εkm

(6.132)

, so that the stress at step (n + 1) is

(n)

(n+1)

= σij + Cijkm εkm

p(n+1)

− Cijkm εkm

(6.133) Similar procedure should be applied to other variables of the model, such as the back stress to account for the evolution of that variable. Figure 6.26 illustrates this algorithm in the multidimensional stress space. Let the yield surface at step (n) be (n) f σij , κ (n) = 0

© 2005 by Chapman & Hall/CRC Press

(6.134)

308

Continuum Mechanics and Plasticity T(n + 1)

(n+1)

Plastic Corrector

(n)

f ((n + 1)) = 0

f ((n)) = 0

FIGURE 6.26 The return-mapping algorithm in the multidimensional stress space. (n)

(n+1)

so that σij is on the yield surface. If σij

is inside the surface, such that

(n+1) (n) f σij ,κ 0 ,κ f σij

(6.136)

then, the return-mapping algorithm ensures that it is lying on the yield surface corresponding to step (n + 1), that is, (n+1) (n+1) f σij ,κ =0

(6.137)

In this case, dλ > 0, which can be determined by substituting (6.133) and the ﬂow rule into (6.137) and solving the resulting equation for dλ. Additional information about the return-mapping algorithm may be found in Simo and Hughes [32]. It sufﬁces to mention that, for associative plasticity with convex yield surfaces, the plastic corrector phase of the algorithm has the unique property that it yields the so-called closest point projection.

6.7

Combined Axial–Torsion of Strain-Hardening Materials

We consider a thin-walled tube made of strain-hardening metal. The coordinate system is chosen so that the radial direction is denoted by 1, the hoop

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

309

direction is 2, and the axial direction is 3. The Mises yield criterion will be used together with three cases of strain-hardening rule: the isotropic hardening, the kinematic hardening, and the combined isotropic–kinematic hardening. We will ﬁrst derive the equations for axial tension and pure torsion, and then present, in Example 6.6, the case in which the tube is ﬁrst subjected to torsion into the plastic range and then subjected to tension while holding the shear stress constant. This problem will be referred to as the tor–ten stress path in this book. We would like to ﬁnd and compare the plastic strains developed due to this loading history using different strain-hardening rules. The yield function is f = ξijD ξijD − 2k 2 = 0

with ξijD = σij − αijD

(6.138)

where shear yield stress which is related to the tensile yield stress by √k is the D Y = 3k. αij is the deviatoric part of back stress αij and ξijD is the deviatoric part of ξij . Using the isotropic–kinematic-hardening parameter β introduced in (6.83), the isotropic-hardening rule is dY = βh d¯ε p

(6.139)

where d¯εp is the equivalent plastic strain increment deﬁned by (6.60). The linear kinematic-hardening rule is p

dαijD = 23 (1 − β)h dεij

(6.140)

and the ﬂow rule is p

dεij = dλ ξijD

(6.141)

In the uniaxial tension, the deviatoric stress, plastic strain increment, and the deviator of the back stress are −σ 3 [σ ] = 0 0 −α

3 [α D ] = 0 0

0 −σ 3 0 0 −α 3

© 2005 by Chapman & Hall/CRC Press

0

0

0 , 2σ 3

−dεp 2 [dεp ] = 0 0

0 −dε p 2 0

0 , 0 dε p

0

0 2α 3

(6.142)

310

Continuum Mechanics and Plasticity

Substituting (6.142) into (6.138), we obtain σ =Y+α

(6.143)

In the case of uniaxial tension, we have from (6.60) and (6.142) 1/2 2 −dε p 2 p 2 (dε ) + 2 = dε p d¯ε = 3 2 p

(6.144)

Thus, dY = βh dεp

(6.145)

Using (6.140) and (6.142), the 33 component equation is 2 3 dα

= 23 (1 − β)h dε p

(6.146)

Therefore, dα = (1 − β)h dεp

(6.147)

Substituting (6.145) and (6.147) into the differential of (6.143), we obtain dσ = h dεp

(6.148)

This equation describes the tensile stress–strain curve for a linear-hardening material independent of the hardening rule. In the torsion of the tube, the deviatoric stress, plastic strain increment, and the deviator of the back stress are

0 [σ ] = 0 0

0 0 τ

0 τ , 0

0

0 [dεp ] = 0

0 0 dγ p 2

0

dγ p 2 , 0

0 [α D ] = 0 0

0 0 α

0 α 0

(6.149) Using (6.149), the yield function reduces to τ =k+α

(6.150)

dγ p d¯εp = √ 3

(6.151)

From (6.60) we have

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

311

and the isotropic-hardening rule is from (6.139) dγ p dY = βh √ 3

or

dk =

βh p dγ 3

(6.152)

The 23 component equation of (6.140) is now dα = 13 (1 − β)h dγ p

(6.153)

The differential form of (6.150) is then obtained as dτ = 13 h dγ p

(6.154)

This equation √ describes the shear stress–strain√curve. We note that if the shear stress is 3τ and the shear strain is dγ p / 3, then (6.154) and (6.148) have the same slope h. Study the tor–ten stress path using the Mises yield criterion with hardening rules given by β = 1, 0, and 0.5.

EXAMPLE 6.6

Solution We use the return-mapping algorithm in this calculation and consider a hypothetical material with shear modulus µ = 26.2 GPa and the initial shear yield stress k = 6.35 MPa. In all three cases, that is, β = 1, 0, and 0.5, we obtain the same shear stress–strain curve shown in Figure 6.27. The slope of the tensile stress–strain curve is assumed to be h = µ/40. The ﬁrst phase of the tor–ten path is in pure torsion and the phase ends when the shear strain γ = 0.01 and the corresponding shear stress τ is 8.47 MPa. At this point, denoted by A in Figure 6.28(a) to (c), the current shear yield stress k is 8.46 MPa for β = 1, 6.35 MPa for β = 0, and 7.41 MPa for β = 0.5; the

Shear Stress , (MPa)

12 10 8 6 4 2 0.005

0.01

0.015

Shear Strain FIGURE 6.27 The shear stress–strain curve for Example 6.5.

© 2005 by Chapman & Hall/CRC Press

0.02

312

Continuum Mechanics and Plasticity

equivalent plastic strain ε¯ p is 0.0056 for all three cases; and the shear back stress α23 is 0 for β = 1, 2.13 MPa for β = 0, and 1.47 MPa for β = 0.5. During the second face of the stress path, AB, the shear stress is kept constant at σ23 = 8.47 MPa, while the axial strain ε increases. The corresponding axial stress σ33 will increase as ε increases. Point B in Figure 6.28(a) to (c) corresponds to ε = 0.012. The quantities σ33 , α33 , α22 , α23 , k, ε¯ p , and γ need to be updated, and dγ p and dε p need to be calculated at each step. Several points along stress-path AB have been chosen for study. The corresponding

(a)

3 23 MPa 30

20

p

dij B

A 10

O a

(b)

(c)

3 23 MPa 30

20

10 b

33 MPa

30

c d e

f

3 23 MPa 30

20 20 A 10 a

p

dij

p

dij b

cd

10

A

e f g B h 20

O

B 10

30 33 MPa

O

ab 10

efg h cd 20

30 33 MPa

FIGURE 6.28 Tor–ten path showing evolutions of yield locus and direction of plastic strain increment for three hardening rules: (a) β = 1, (b) β = 0, and (c) β = 0.5.

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

313

TABLE 6.1 Yield Loci and Direction Angles of Plastic Strain Increments β=1 Yield locus fb fc fd fe ff fg fh

β=0

ε

θ (◦ )

0 0.001 0.005 0.01 0.012

90 37.5 32.9 28.5 26.9

β = 0.5

ε

θ (◦ )

ε

θ (◦ )

0 0.001 0.0025 0.005 0.0075 0.01 0.012

90 58.3 47.7 36.9 30.0 24.8 22.0

0 0.001 0.0025 0.005 0.0075 0.01 0.012

90 61.4 51.1 43.3 37.2 32.7 29.5

yield loci fa , fb , fc , etc. passing through these points are shown in the ﬁgures and are denoted by a, b, c, etc. The yield loci denoted by letter a are the initial yield loci in all three cases. Yield loci with corresponding ε values are listed in Table 6.1. It is clear from Figure 6.28(a) that the yield locus expands centering at the origin O for isotropic hardening. In the case of kinematic hardening, shown in Figure 6.28(b), the yield locus keeps the original size but moves while the tor–ten stress path is pursued. Figure 6.28(c) shows a case of combined isotropic–kinematic hardening with β = 0.5. In this case, the yield locus both expands and moves. The short inclined lines in the ﬁgures show √ p the directions of dεij with components ((dγ p / 3), dεp ). An angle √ p 180 −1 dγ / 3 θ= tan π dε p p

(a)

which is the inclined angle of dεij is deﬁned. At the beginning of the stress path at A, θ = 90◦ for all three cases. In the case of β = 1, θ decreases to 37.5◦ at ε = 0.001 and continues to decrease as ε increases and θ = 26.9◦ at point B. In the case of β = 0, θ decreases to 58.3◦ at ε = 0.001 and continues to decrease as ε increases and θ = 22.0◦ at point B. In the case of β = 0.5, θ decreases to 61.4◦ at ε = 0.001 and continues to decrease as ε increases and θ = 29.5◦ at point B. These angles are listed in Table 6.1. In all cases the directions are normal to the corresponding yield loci. It is evident that different hardening rules lead to different plastic strains. Figure 6.29 plots σ33 versus ε during the stress-path AB. It is seen that the three cases of strain-hardening lead to very different stresses. Isotropic hardening (β = 1) leads to the highest stress of the three cases. This effect can also been seen directly from Figure 6.28(a). The strain paths corresponding to stress-path AB are shown in Figure 6.30. The case of β = 0.5 leads to the highest shear strain. We know that the shear strain has started from the prestrain value of 0.01 during this tension phase. But, the increase in the shear

© 2005 by Chapman & Hall/CRC Press

314

Continuum Mechanics and Plasticity

Axial Stress, (MPa)

30

=1

25 20

= 0.5

15

=0

10 5

0.002 0.004 0.006 0.008 Axial Strain

0.01 0.012

FIGURE 6.29 Axial stresses for tor–ten path.

Shear strain

0.03

= 0.5

0.025 =0 0.02 =1

0.015

0.002 0.004 0.006 0.008 Axial strain

0.01 0.012

FIGURE 6.30 Strain paths for tor–ten path.

strain is still larger than the increase in the tensile strain for cases involving kinematic hardening and the increase is about the same as the increase in the axial strain for the isotropic-hardening case.

6.8

Flow Theory in the Strain Space

The ﬂow theory of plasticity previously presented has been formulated in the stress space. The state of stress is represented by a point in this space and is sometimes referred to as the stress point. If this stress point is located within the yield surface, the material is in the elastic state; and if the stress point is on the yield surface, the material is in the plastic state. The yield surface is deﬁned by a function of stress and other parameters, and the yield surface can expand, distort, or move in the stress space. When the material is in its plastic state, plastic ﬂow occurs according to a ﬂow rule, which deﬁnes the direction and magnitude of the plastic strain increment. Therefore, in this formulation, the stress is the independent variable and the plastic strain

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

315

B A

C D

E

O

FIGURE 6.31 Stress–strain curve of a strain-softening material.

rate (or increment) is the dependent variable. This formulation of plasticity works well for metals and generally works well for strain-hardening materials deﬁned in Drucker’s sense, see Section 6.5. Some materials, such as geotechnical materials (soils, concretes, rocks, ice, etc.) are strain-softening materials. The axial stress–strain curve for this type of materials has a positive slope initially. But, after it reaches a peak, the slope turns into negative. In the region of negative slope, plastic deformation continues with decreasing stress. Figure 6.31 shows a schematic stress–strain curve of a strain-softening material. The stability of strain-softening materials is deﬁned by an Ilyushin postulate [33], which states that the work done by external forces on a material over a closed cycle of strain is positive. In this postulate, work is done over a cycle of strain rather than a cycle of stress as is in Drucker’s postulate. Drucker’s postulate is more restrictive than Ilyushin’s postulate. Referring to Figure 6.31, Drucker’s postulate says that area ABCDA is positive, but Ilyushin’s postulate says that area ABCEA is positive. Ilyushin used strain as an independent variable and stress was a response. He proposed a yield function in the strain space [34] but much of his effort was related to characterizing the stress response to a predetermined strain path. Ilyushin’s work is further discussed in Chapter 7. A ﬂow theory of plasticity expressed in the strain space was proposed by Naghdi and Trapp [35]. Casey and Naghdi [36] further showed that the stress space formulation is a special case of the strain space formulation. In the strain space formulation, the stress response is given by the constitutive equation p

σij = σij (εrs , εrs , κ)

(6.155) p

where κ is the work-hardening parameter. At ﬁxed values of εij and κ, p (6.155) may be inverted to obtain εij as a function of σij , εij , and κ. The yield function (or loading function) in the strain space is p

g(εij , εij , κ) = 0

© 2005 by Chapman & Hall/CRC Press

(6.156)

316

Continuum Mechanics and Plasticity

which corresponds to yield function p

f (σij , εij , κ) = 0

(6.157)

in the stress space. The ﬂow rule is p

ε˙ ij = λρij

∂g ε˙ rs , ∂εrs

if g = 0

and

∂g ε˙ rs > 0 ∂εrs

(6.158)

where λ and ρij are, respectively, a positive scalar-valued function and a p nonzero symmetric tensor-valued function of εij , εij , and κ. If the evolution of κ is p

κ˙ = βij ε˙ ij

(6.159)

then, by use of the consistency condition, it may be shown that (∂f /∂σij )σ˙ ij ∂f ∂g = 1 − λξ (∂g/∂εrs )˙εrs ∂σij ∂εij

(6.160)

p

where ξ is a nonnegative function of εij , εij , and κ. It is seen from (6.160) that the loading conditions in the two spaces are not equal during loading. However, they are equal during unloading and neutral loading. Extensive experimental work has been carried out to determine yield surfaces in the stress space, which is discussed in Chapter 7. Little has been reported concerning experimental determination of yield surfaces in the strain space. But, according to Naghdi and his coworkers [35,36], the yield surface in the stress space can be transformed into the strain space.

6.9

Remarks

We have presented in this chapter the fundamental concept of the ﬂow theory of plasticity. All main elements of the theory have been presented in their simplest forms. We have considered no distortion of the yield surface and the associated ﬂow rule (with normality condition) is used in its simplest form. The isotropic hardening, the kinematic hardening, and the combined isotropic–kinematic hardening have been discussed together with a nonlinear rule of kinematic hardening. In a simplest multiaxial case, the case of combined axial–torsion presented in Section 6.7, we compare results of this simple ﬂow theory using three hardening rules. We have shown that, using this simple model, all three hardening rules lead to the same results for uniaxial tension and pure torsion, but the results for combined axial–torsion vary greatly with the hardening rule assumed. The ultimate question is how

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

317

valid these results are. They show a wide range of differences, and apparently only one of them, or maybe none of them, are correct. In order to establish the validity of a model, the results need to be veriﬁed by experimental ﬁndings. It is the purpose of Chapter 7 to discuss experiments aiming at providing experimental facts that can be used to verify, improve, and reﬁne the theory of plasticity. We will discuss some recently formulated theories and also discuss ideas that extend the theory of plasticity into the ﬁnite strain range.

References 1. Taylor, G.I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc. A. 230, 323, 1931. 2. Bertsch, P.K. and Findley, W.N., An experimental study of subsequent yield surfaces-corners, normality, Bauschinger effect and allied effects, Proc. 4th U.S. Natl. Cong. Appl. Mech., 893, 1962. 3. Mair, W.M. and Pugh, H.L.D., Effect of prestrain on yield surfaces in copper, J. Mech. Eng. Sci., 6, 150, 1964. 4. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Struct., 8, 463, 1972. 5. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 6. Wu, H.C. and Ho, C.C., Strain-hardening of annealed 304 stainless steel by creep, J. Eng. Mat. Tech., 115, 345, 1993. 7. Ishikawa, H., Subsequent yield surface probed from its current center, Int. J. Plasticity, 13, 533, 1997. 8. Szczepinski, W., On the effect of plastic deformation on yield criterion, Arch. Mech., 15, 276, 1963. 9. Batdorf, S.B. and Budiansky, B.A., A mathematical theory of plasticity based on the concept of slip, NACA, TN 1871, 1949. 10. Lin, T.H., A proposed theory of plasticity based on slips, Proc. Second U.S. Natl. Congress Appl. Mech., 461, 1954. 11. Lin, T.H., On stress–strain relations based on slips, Proc. Third U.S. Natl. Congress Appl. Mech., 581, 1958. 12. Phillips, A., A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity, 2, 315, 1986. 13. Mises, R. von, Mechanik der Fasten Korper im plastisch defomablen Zustand, Göttingen Nachrichten, Math. Phys. Kl., 581, 1913. 14. Tresca, H., On the ﬂow of solid bodies subjected to high pressure, C.R. Acad. Sci. Paris, 59, 754, 1864. 15. Lode, W., Versuche über den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle, Eisen, Kupfer und Nickel, Z. Phys., 36, 913, 1926. 16. Hill, R., The Mathematical Theory of Plasticity, Clarendon Press, Oxford, 1950, 38. 17. Hundy, B.B. and Green, A.P., A determination of plastic stress–strain relations, J. Mech. Phys. Solids, 3, 16, 1954. 18. Lianis, G. and Ford, H., An experimental investigation of the yield criterion and the stress–strain law, J. Mech. Phys. Solids, 5, 215, 1957.

© 2005 by Chapman & Hall/CRC Press

318

Continuum Mechanics and Plasticity

19. Phillips, A. and Moon, H., An experimental investigation concerning yield surfaces and loading surfaces, Acta Mech., 27, 91, 1977. 20. Ohashi, Y., Kawashima, K., and Yokochi, T., Anisotropy due to plastic deformation of initially isotropic mild steel and its analytical formulation, J. Mech. Phys. Solids, 23, 277, 1975. 21. Drucker, D.C., A more fundamental approach to plastic stress–strain relations, in Proc. 1st U.S. Natl. Congress Appl. Mech., ASME 487, 1951. 22. Bell, J.F., The experimental foundations of solid mechanics, Handbuch der Physik, Via/1, Flügge, Ed., Springer, Berlin, 1973. 23. Prager, W., The theory of plasticity: a survey of recent achievements ( James Clayton Lecture), Proc. Inst. Mech. Eng., 169, 41, 1955. 24. Hodge, Jr., P.G., Piecewise linear plasticity, Proc. 9th Int. Congress. Appl. Mech., 8, 65, 1957. 25. Ziegler, H., A modiﬁcation of Prager’s hardening rule, Quart. Appl. Math., 17, 55, 1959. 26. Armstrong, P.J. and Frederick, C.O., A mathematical representation of the multiaxial Bauschinger effect, G.E.G.B. Report RD/B/N 731, Berceley Nuclear Laboratories, 1966. 27. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 28. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 29. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 30. Prager, W., Recent developments in the mathematical theory of plasticity, J. Appl. Phys., 20, 235, 1949. 31. Drucker, D.C., A deﬁnition of stable inelastic material, J. Appl. Mech., 26, 101, 1959. 32. Simo, J.C. and Hughes, T.J.R., Computational Inelasticity, Springer-Verlag, New York, 1998. 33. Ilyushin, A.A., On the postulate of plasticity, PMM, 25, 503, 1961. 34. Ilyushin, A.A., Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 196, 1963. 35. Naghdi, P.M. and Trapp, J.A., The signiﬁcance of formulating plasticity theory with reference to loading surfaces in strain space, Int. J. Eng. Sci., 13, 785, 1975. 36. Casey, J. and Naghdi, P.M., On the nonequivalence of the stress space and strain space formulations of plasticity theory, J. Appl. Mech., 50, 350, 1983.

Problems (1) Acylindrical specimen is loaded in tension from 0 to a stress of 500 MPa and has undergone a strain of 0.2 at this point. This point is denoted by A in Figure 6.32. Unloading then occurs following a curve as shown in the ﬁgure. Determine the yield point during unloading, if yield is deﬁned by a proof strain of (a) 0.1%, (b) 0.5%, or (c) 1.0%. Assuming that the yield surface remains circular after prestrain in the two-dimensional principal stress space, sketch the yield

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

319 Stress MPa

A

500 400 300 200 100 0.18

Strain

0.17

0.19

0.20

–100 –200 FIGURE 6.32 Figure for Problem 1.

T L

S

S

A

u

P FIGURE 6.33 Figure for Problem 2.

surfaces corresponding this state of stress using the yield stresses previously determined based on different amounts of proof strain. (2) Consider the three-bar truss shown in Figure 6.33. All bars have the same cross-sectional area A0 and are made of an elastic-perfectly plastic material. Due to the application of force P, the displacement at A is u downward. Assume that the deformation is small so that u/L 1. Determine displacement u, the stresses σT and σS in bars T and S, respectively, and the corresponding strains εT and εS , expressed in terms of p = P/A0 . Plot the p versus u/L diagram. (Hint: Consider the elastic phase, the end of the elastic phase when the ﬁrst bar yields, the elastic–plastic phase, and the end of this second phase.)

© 2005 by Chapman & Hall/CRC Press

320

Continuum Mechanics and Plasticity

(a)

(b) B

A E

O

O

C

D FIGURE 6.34 Figure for Problem 3.

(3) Figure 6.34(a) shows a sketch of uniaxial loading–unloading–reloading curve. Assume that the material obeys Mises yield criterion with kinematic hardening. Sketch in Figure 6.34(b) the yield surfaces that correspond to the stress states of A, B, C, D, and E. Figure 6.34(b) describes the shear versus axial stress space in the combined axial–torsion of a thin-walled tube. (4) A long cylindrical pressure vessel is made of a metal with shear yield stress of k = 560 MPa and the maximum internal pressure during use is limited to 35 MPa. Considering the middle section of the vessel away from the ends, if no section of the vessel is to yield according to the Mises yield criterion, determine the required wall thickness if the outer radius is 600 mm. (5) A closed-ended thin-walled tube is subjected to an axial tensile force F, which is less than F0 necessary to cause yielding. Apply a gradually increasing internal pressure p and determine p expressed in terms of F when yielding occurs. Use Mises yield criterion and denote the wall thickness by t and the mean radius of the tube by r. (6) A metal of yield stress Y = 300 MPa is subjected to a principal stress state of (σ1 , σ2 = −0.2σ1 , σ3 = 0.5σ1 ). If the stress ratios remain constant as the stresses increase, determine σ1 at yielding using the Mises yield criterion. (7) Derive (6.12). (8) Derive (6.13). (9) In a biaxial tension–compression test of perfectly-plastic material, (a) sketch the Mises yield locus, if Y = 250 MPa; ﬁnd the components of the plastic strain increment at the loading point speciﬁed by (b) σx = 250 MPa and σy = 250 MPa; and (c) σx = −100 MPa and σy = 184.52 MPa. √ (10) Find the expression of equivalent stress σ¯ = 3/2{σij σij }1/2 in the case of uniaxial stress. (11) Find the expression of equivalent plastic strain increment d¯εp 2 {dε p dε p }1/2 in the case of uniaxial tension. ij ij 3

© 2005 by Chapman & Hall/CRC Press

=

The Flow Theory of Plasticity

321

(12) What is the deﬁnition of a convex function? p

(13) If the yield function is f = f (σij − c(κ1 )εij ) = κ0 , where κ0 = constant and p

p

κ˙ 1 = (˙εkm ε˙ km )1/2 , assume that the normality condition holds, show that the ﬂow rule is −(∂f /∂σkm )(∂f /∂σij )dσkm

p

dεij =

p

(∂f /∂σrs )(∂f /∂εrs ) + [(∂f /∂σrs )(∂f /∂σrs )]1/2 (∂f /∂κ1 )

(14) Using the equations of Problem (13), show that for Mises’s yield criterion, the ﬂow rule is p

dεij =

(∂f /∂σkm )(∂f /∂σij )dσkm p 2cκ0 + 2κ0 (∂c/∂κ1 )εrs (∂f /∂σrs )

(15) In the case of uniaxial stress, show that the ﬂow rule of Problem (14) reduces to dσ = Et dεp . Determine the expression of Et .

© 2005 by Chapman & Hall/CRC Press

7 Advances in Plasticity

7.1

Introduction

We discussed the basic concepts and formulation of plasticity in Chapter 6. With this knowledge we are ready to explore what other possibilities are there to improve the theory of plasticity. In fact, a great deal of work has been done since 1950 aiming to observe and understand plastic deformation and the mechanics of it. More realistic constitutive models have been proposed. While signiﬁcant progress has been made, still more research work is desirable if the constitutive modeling of plastic deformation is to keep pace with the ever advancing technologies, methods, and equipment of computation. We are currently in a situation where high-powered computational mechanics is using concepts of plasticity that are basic and unsophisticated. The requirement for accuracy of the simulated results will go hand-in-hand with the requirements for safety, efﬁciency, and cost reduction such as reducing the wastes of manufacturing, as various related industries advance. The sophistication of constitutive modeling holds the key to this accuracy requirement. We would like to emphasize that the task of improving the constitutive modeling depends signiﬁcantly on experimental ﬁndings. The experiments will guide the development of theories and theoretical investigation will in turn suggest new experimental conditions. In this chapter, we attempt to describe the state of the art in terms of the experiments which are carried out to improve constitutive modeling. In the theoretical developments, two approaches have been taken by researchers: the traditional plasticity approach with its improvements and a plastic strain trajectory approach, in which the stress depends on the plastic strain trajectory. The traditional plasticity approach is stress-controlled. The stress is the input and the strain is the response. In this approach, we propose a yield function in the stress-space, a ﬂow rule which is usually related to the stress and/or stress increment, and a strain-hardening rule with the back stress moving in the stress space. We discuss in this chapter some modern works belonging to this group. In the plastic strain trajectory approach, the plastic strain path is the input and the stress is found as a response. The relationship between the plastic strain trajectory and the stress is established 323

© 2005 by Chapman & Hall/CRC Press

324

Continuum Mechanics and Plasticity

through a functional or a modulus, depending on whether the constitutive equation is in an integral form or in a differential form. The two forms are equivalent if the boundary conditions are speciﬁed. This approach, including the endochronic theory of plasticity by Valanis [1,2], is brieﬂy described in this chapter. The endochronic theory, which has been derived from the thermomechanical theory of internal state variables, is fully discussed in Chapter 8. We discuss in this chapter how a constitutive equation may be extended to the ﬁnite deformation range. The concept of material objectivity discussed in Chapter 4 must be applied. Appropriate stress and strain measures and their rates should be used. Finally, material texture will develop as plastic deformation proceeds, resulting in material anisotropy. How can the change of material texture be described at the phenomenological level? We attempt to provide research results which address the aforementioned questions.

7.2

Experimenal Determination of Yield Surfaces

The ﬂow theory of plasticity is built upon the concept of yield surface, and therefore yield surface is by far the most important element of all the elements of the theory. We have already discounted Tresca’s yield criterion in the Chapter 6 and concentrated on the Mises yield criterion. But how valid is the Mises yield criterion? Generally speaking, it is a good approximation for initial yield surface (see Section 6.2), although some deviations, such as those shown by Ohashi and Tokuda [3], have been reported. The evolution of the yield surface is of interest to many researchers. As was mentioned in Section 6.2, the size and shape of subsequent yield surfaces depend greatly on the deﬁnition of yield. The yield Surface C of Figure 6.3 determined by the method of backward extrapolation encloses a large elastic region which lies outside of Surfaces B and A. If we insist that the region inside the yield surface is elastic, then the strain is elastic at any point in this region if Surface C is considered as the yield surface. But the same point is outside Surfaces B and A, and therefore, referring to Surfaces B and A, plastic deformation would occur. Apparently, plastic strain is being neglected if Surface C is considered as the yield surface. The quest for more accurate descriptions of the plastic behavior calls for a proportional limit (or small proof strain) deﬁnition of yield, and the challenge is to determine how the yield surface evolves when the material is subjected to various loading histories. These experiments determine the yield function and the back stress which is the center of the yield surface. These are two pieces of information that are central to the ﬂow theory of plasticity. The study of evolution of yield surface has led to the improvements of the theory of plasticity. The effect of various deﬁnitions of yield on the size and shape of subsequent yield surfaces has been previously mentioned. Other factors that affect the determination of yield surface have been discussed by Wu and Yeh [4] and these factors are discussed next (following [4], with permission from Elsevier). © 2005 by Chapman & Hall/CRC Press

Advances in Plasticity 7.2.1

325

Factors Affecting the Determination of Yield Surface

Due to the availability of closed-loop, servo-controlled hydraulic testing machines with sophisticated computer-controlled circuits, it is even more appropriate than ever to discuss some of the factors affecting the determination of yield surface. In earlier test machines, either deadweight or mechanical, “experience” of the investigator was often an important factor in obtaining “reasonable” yield surfaces. With the use of a closed-loop test machine, the “experience” of an investigator can apply only before the beginning of a test or after a test has been completed and no in-between adjustment can be made during the test to smooth out the data. Therefore, it is likely that more data scatter is observed when a closed-loop machine is used, see Phillips and Lu [5]. These data represent more closely the experimental results in their raw form. The deﬁnition of yield by means of a 5µ equivalent plastic strain has gained popularity in the recent literature. One of the reasons for the popularity is that the deﬁnition of yield of 5µ is close to that based on the proportional limit and, therefore, one specimen may be used to determine the initial and all of the subsequent yield surfaces. Astrain of 5µ is, however, a very small strain measured by resistance strain gauges, and there are factors that affect the experiment and may cause a variation of several microstrains. Thus, 5µ is a very sensitive deﬁnition of yield and the resulting data scatter is to be expected. Even though the yield point is based on a proof strain of 5µ, it must be mentioned that the actual plastic strain incurred before a yield point can be conﬁrmed is approximately 10µ. This amount depends on the technical details used by the investigator. The factors presented in the following subsections should be considered in connection with the determination of yield surfaces.

7.2.1.1 The elastic modulus and the zero offset strain For an accurate determination of plastic strain, the “zero offset strain” as shown in Figure 7.1(a) and denoted by ε R should be accounted for. In the ﬁgure, the circular dots represent acquired data for a one-dimensional stress–strain curve and the straight line is an approximation determined by the least mean-square method, using some selected data in the elastic region. Accordingly, the axial plastic strain, ε p , can be determined by εp = ε − ε R −

σ E

(7.1)

where ε is the axial strain; σ is the axial stress; E is Young’s modulus, which is the slope of the straight line, and εR the zero offset strain. The quantity ε R is measured by intersecting the straight line with the ε-axis and is therefore related to the value of E. Ideally, εR should be zero. However, due to the nature of the servo-controlled machine and the time interval of data acquisition, the data will scatter somewhat (exaggerated to show the effect) as shown in Figure 7.1(a). Therefore, some amount of ε R is bound to be present. © 2005 by Chapman & Hall/CRC Press

326

Continuum Mechanics and Plasticity (a)

(b)

P

Y B D

A R

∆p

/E

O

(c)

R

100 c

Shear Stress (MPa)

80

60

d

a

p e

40

20 o 0

b 10 20 30 40 50 60 Axial Stress (MPa)

FIGURE 7.1 (a) Zero offset strain, (b) strain domain Dε , (c) effect of probing path (From Wu, H.C. and Yeh, W.C., Int. J. Plasticity, 7, 803, 1991. With permission from Elsevier).

The accuracy and the numerical value of the elastic modulus are highly dependent upon the number of data points used in the least square analysis. A different number of data points leads to different values for the elastic modulus, and also leads to different initial zero offset strains. The zero offset strain is shown in (7.1) to affect the amount of proof strain. This effect is quite signiﬁcant, especially when the proof strain is as small as 5µ. In an effort to estimate the range of variation in the elastic modulus and the zero offset strain with respect to the number of data points used in the least square analysis, a strain domain, Dε , is deﬁned in the strain space and shown as AB in Figure 7.1(b). Data points lying between A and B are used in the least square analysis. All data points of this domain are within the elastic region. OP represents a probing path of proportional straining on which a

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

327

yield point Y is to be determined. Point O indicates the point from which the probe emanates, and it may differ from the strain-free origin in the case when subsequent yield surfaces are to be determined. Considering a pure torsion test, Wu and Yeh [4] found that ε R varies up to 5µ when Dε is < 0.01%, but the variation is still 2 to 3µ even with Dε >0.01%. This amount of variation is large indeed when the deﬁnition of yield is set at 5µ. Adding to the complication is the fact that the slope of elastic loading associated with probes of different paths may be slightly different from one another. This was experimentally veriﬁed by Ivey [6] and Wu and Yang [7]. Ivey reported that when a specimen of 2024-T4 aluminum was subjected to prestrain in tension followed by a pure torsion while keeping the tensile strain constant, the shear modulus varies by an amount depending upon the magnitude of the prestrain in tension. Wu and Yang found that, for a one-dimensional tension–compression test, the slope of the unloading curve at various strain was not quite the same levels for both 6061-T6 aluminum and 4142 steel. Thus, the elastic modulus and the zero offset strain ε R vary from one probe to the other, and their magnitudes should be determined for each path. However, this is usually not practical and not accounted for in the experiments. Therefore, this effect contributes to the data scatter of yield surfaces.

7.2.1.2

The effect of strain domain on the yield stress

As the elastic modulus and the zero offset strain are affected by Dε , the equivalent plastic strain is affected through an equation similar to (7.1). Consequently, the yield stress thus determined is also affected. The yield stress determined in the previously mentioned pure torsion test with varied Dε but a constant Rε of 0.01% shows severe ﬂuctuations when the strain domain Dε is very small, and it becomes steady when Dε is greater than approximately 0.01%.

7.2.1.3 The effect of probing path In order to minimize the effect of probes, consecutive probes are chosen not to be on the same side of the yield surface. Yet, the effect of probes is still signiﬁcant in that radial and nonradial probing paths do not lead to consistent yield points. This assertion is substantiated by the results of an experiment involving strain paths oa, obc, and ode illustrated by Figure 7.1(c). In the radial probe oa, the yield point was determined at “a” and any point beyond this point is in the postyielding state. Consequently, the point “p” of the line “bc” is considered to be in a yielded state. However, as judged by the probe of nonradial path obc, this particular point “p” was still in the elastic region. Point “c” was the yield point for this path. The yield point of path ode was determined to be at e. Figure 7.1(c) has thus demonstrated the probing path dependence of the yield point when it is determined by a small proof strain of 5µ.

© 2005 by Chapman & Hall/CRC Press

328

Continuum Mechanics and Plasticity

7.2.1.4 The effect of strain rate in probing It is known that some metallic materials exhibit signiﬁcant strain-rate effect even at room temperature, as mentioned in Section 5.2.4. The experimental constant strain-rate stress–strain curves show that stresses at different strain rates are signiﬁcantly unequal only in the postyielded range and thus a large offset strain deﬁnition of yield would lead to a yield stress which is quite strain-rate dependent. However, a rather weak rate sensitivity is evident when a small proof strain is used. It is thus reasonable to assume that for a proof strain as small as 5µ, the strain-rate effect in the probing is negligible. A similar conclusion was drawn by Ellis et al. [8] in connection with their testing of 316 stainless steel. For the range of probing rate (100 to 500 µε/min) used, the writers concluded that the probing rate had little effect on yield behavior and that the difference in size and position of the yield surfaces they determined was more related to the sequence in which the yield surfaces were determined rather than the probing rate.

7.2.2

A Summary of Experiments Related to the Determination of Yield Surfaces

Extensive literature is available on the issue of experimental determination of yield surfaces, with prestrains (i.e., specimen subjected to strain before a yield surface is determined) within the strain range (2% or less) of an electricalresistance strain gauge. The experimental works described here were carried out at room temperature. Most experiments were conducted using thinwalled tubes subjected to combined tension and torsion. This group includes Taylor and Quinney [9], Naghdi et al. [10], and Ivey [6] with prestrain in torsion; McComb [11] with prestrain in tension; Mair and Pugh [12] with prestrain in tension, partially unloaded and then strained in torsion; Bertsch and Findley [13] with zigzag paths in small steps; Phillips and Moon [14], Phillips and Lu [5], Shiratori et al. [15], and Ishikawa [16] with various prestrain histories; Wu and Yeh [4] with proportional paths of loading-unloading-reloading-cyclic steady state. Experiments were conducted by Lode [17] and Hu and Bratt [18] using thin-walled tubes subjected to tension and internal pressure. Plate specimens were used by Szczepinski [19], Szczepinski and Miastkowski [20], and Shiratori and Ikegami [21]. The experimental results generally conﬁrmed that the initial yield surface is closed to the Mises ellipse and the subsequent yield surfaces are obtained from the expansion in size, the motion, and distortion of the Mises ellipse. If the yielding is deﬁned using a small (5 to 10µ) proof strain, then the size of the ellipse does not change, that is, no cross effect has been observed. The discussion in this section is devoted to the effect of loading path on the yield surface, which includes the stress-controlled path and the strain-controlled path. The path may be linear or nonlinear, and a proportional strain path may not lead to a proportional stress path depending on material tested.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

329

(2)

(6)

(7) (3)

A

(5)

B

(4)

(1) O

D

C

FIGURE 7.2 Loading paths for combined axial–torsion.

7.2.2.1 Proportional path The proportional path includes monotonic axial loading, path (1) of Figure 7.2, monotonic torsion loading, path (2), and proportional combined tension and torsion, path (3). Most early works reported in the literature were conducted using load-control machines and were therefore controlling the stress path. Servo-controlled hydraulic test machines have been used in more recent works and stress- or strain-controlled tests are possible. Both cases (i.e., stressor strain-control) lead to the same result for monotonic axial loading and monotonic torsion in the small strain range. Phillips and Tang [22], Ishikawa [16], and most experiments reported in the literature used a prestress path. Wu and Yeh [4] used prestrain paths for monotonic axial and monotonic torsion prestrains, but a prestress path for a combined tension and torsion proportional loading. A conclusion arrived at from all available experimental data is that the yield surface undergoes kinematic hardening along the direction of loading and gets distorted with the “ﬂattened rear part” of the yield surface facing the origin of the stress space. The extent of kinematic hardening and the amount of isotropic hardening depend√upon the material tested and upon the deﬁnition yield. Thus, if plotted in the 3τ versus σ space, where τ is the shear stress and σ the axial stress, the initial yield surface for an initially isotropic material is a circle and the subsequent yield surfaces can be approximately described by ﬂattened ellipses. In a combined tension–torsion proportional loading, the initial yield surface, which is a circle, will gradually become distorted as the prestrain increases, with the ﬂattened ellipse facing the origin of the stress space. Note that this ﬂattened ellipse is a result of distortion and not a rotation of the yield surface. In fact, it is fair to say that no rotation of yield surface occurs during proportional loading. Subsequent yield surfaces with proportional prestrains are shown schematically in Figure 7.3. We note that some subsequent yield surfaces in the literature show a “rounded nose” in the direction of prestressing but a ﬂat rear on the side opposite to the prestress (see the solid curves), but some reported experimental yield surfaces do not

© 2005 by Chapman & Hall/CRC Press

330

Continuum Mechanics and Plasticity 3

O

FIGURE 7.3 Subsequent yield surfaces with proportional prestrain.

A

D

C

O

B

FIGURE 7.4 Loading point and yield point.

show these characteristics (see the dashed curves). The reason for differences is related to the point picked as the yield point when reloading takes place in the yield surface probing. Referring to Figure 7.4, the material is ﬁrst loaded from O to A, which moves the yield surface to its current state. Partial unloading from A to B would put the stress point at the center of the current yield surface. BCD represents the probing of the current yield surface and C is the yield point. If point A, which is known as the loading point is considered a point on the yield surface, then the yield surface will show a rounded nose. On the other hand, if C is considered a point on the yield surface, then the yield surface does not show a rounded nose. Some authors [14] distinguish between these two points and consider the ideas of loading surface and yield surface. But most experimental results found in the literature do not make this distinction. In the case of combined axial–torsion, only three papers have reported test results on proportional loading into the large strain range and they are discussed here. Helling et al. [23] conducted stress-controlled tests on several © 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

331

materials and obtained √ data showing the evolution of yield surface up to a shear prestrain of γ / 3 = 0.32 under torsion, path (2) of Figure 7.2. The paper did not specify whether they were free- or ﬁxed-end torsion tests. But since the authors did not report the axial stress during the torsion test, one can assume that the tests were conducted under the free-end torsion condition. The results are similar to those obtained in the small strain range, except that isotropic hardening is signiﬁcant for some materials. The paper did not discuss path (1) — monotonic axial preloading — but it did report a case of proportional loading, path (3), with a result similar to those observed in small strain. The ﬂattened ellipse was facing the origin of the stress space. However, this case was conducted with an effective prestrain of only 5%, which is small. Wu et al. [24] tested annealed 304 stainless steel and determined the initial and subsequent yield surfaces for two loading paths. Path (1) in axial loading had an axial prestrain of 20% and path (2) in free-end torsion had a shear prestrain of 20%. Experimental results showed that both the forward and rear parts deﬂated as the loading proceeded. These results contradict what is known at the small strain level, where the forward part inﬂates. In addition, for a prestrain of only 20%, the cross effect is very signiﬁcant for the material tested. This cross effect was not apparent in the work of Wu and Yeh [4] for the same material at small strain level. The experiments reported in Wu [25] provide another set of test data related to the evolution of yield surface with large prestrains. In the experimental determination of subsequent yield surfaces, a major difﬁculty is that strain gauges used to probe the previous yield surface are no longer functional when subsequent prestrain for the next yield surface exceeds 2%. Since the same specimen is used to determine several subsequent yield surfaces, the sum of all preloading (or prestrains) is the prestrain before next yield surface probing. The method used to overcome this difﬁculty was to unload the specimen after the specimen had been subjected to a predetermined amount of prestrain. The specimen was then removed from the test machine and new strain gauges were installed and cured. The specimen was then mounted again on the test machine and gradually loaded to merge with the stress–strain curve of prestraining, monitored by an axial–torsional extensometer designed and built by Wu and Xu [26]. At this point, a subsequent yield surface was probed using the newly installed strain gauges. The same method was used to determine other subsequent yield surfaces. Experiments were conducted for path (1) up to an axial prestrain of ε = 0.45 and for path (2) up to a shear prestrain of γ = 0.4. The test for path (2) was conducted under the free-end torsion condition. Note remarked that the test data for both paths (1) and (2) enable the determination of a complete set of parameters that can be used to calculate the combined axial–torsion response of the tube. Owing to prestrains into the ﬁnite deformation range, the expansion (or contraction) of yield surfaces is signiﬁcant for the materials tested by Helling et al. [23], Wu et al. [24], and Wu [25], even though yield was determined by a proof strain of 5µ. © 2005 by Chapman & Hall/CRC Press

332

Continuum Mechanics and Plasticity 3 Surface A

Surface B

Initial Yield Surface

O

FIGURE 7.5 Evolution of yield surface for tor–ten path (4).

7.2.2.2 Stress-controlled torsion–tension path Two stress-controlled torsion–tension paths (tor–ten for short) are meaningful. These paths are illustrated in Figure 7.2. Path (4) denotes a path with pretorsion from O to A, followed by an elastic unloading to an approximated center of the current yield surface at B. Axial loading is then applied, keeping the shear stress constant at the value of τB . Path (5) denotes a path with pretorsion from O to A, followed by an axial loading while keeping the shear stress constant at the value of τA . The tor–ten path (4) has been investigated by several investigators, including Phillips and Tang [22], Shiratori et al. [15], Ishikawa [16], and Helling et al. [23]. Figure 7.5 shows schematically the evolution of the yield surface for tor–ten path (4). Test results show that the yield surface (Surface A) at the end of the pretorsion stage serves as the basis for the subsequent yield surfaces (Surface B) generated by tension. The surface ﬂattens without rotation as the axial stress increases. All results have been obtained in the small strain range, including the tests of Helling et al. [23] for this case. No experimental data for the large strain range has been found in the literature for this test. Tor–ten path (5) has been investigated by Helling et al. [23]. The data have been obtained for tests up to a total prestrain (torsion and tension) of only 5%. Test results shows a rotation of yield surface as the axial stress increases. The yield surfaces of path (5) are shown schematically in Figure 7.6. Surface A denotes the yield surface at the end of the pretorsion stage and Surface B the yield surface after tensile stressing has been applied. 7.2.2.3 Stress-controlled tension–torsion path The stress-controlled tension–torsion paths are the counter part of the stresscontrolled tor–ten paths. Results should be similar in nature to those discussed

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

333 3 Surface A Surface B

O Initial Yield Surface

FIGURE 7.6 Evolution of yield surface for tor–ten path (5) (From Helling, D.E. et al., J. Eng. Mater. Technol., 108, 313, 1986. With permission from ASME).

in Section 7.2.2.2. There are two cases: path (6) denotes a path with pretension from O to C (see Figure 7.2), followed by an elastic unloading to an approximated center of the current yield surface at D. Torsion loading is then applied while keeping the axial stress constant at the value of σD . Path (7) denotes a path with pretension from O to C, followed by a torsion loading while keeping the axial stress constant at the value of σC . Path (6) has been investigated by several investigators, including Phillips and Tang [22], Shiratori et al. [15], and Ishikawa [16], and path (7) has been investigated by Helling et al. [23]. These investigations have all been conducted with prestrains in the small strain range. 7.2.2.4

Other paths

Experiments have been conducted following other stress-controlled paths and some with unloading and cyclic loading. However, the investigators were interested in other aspects of plastic behaviors and no information about the corresponding yield surfaces was reported. The investigations associated with the variation of plastic strain increment along a stress path will be discussed in the next section, related to the experimental investigation of the ﬂow rule. Strain-controlled loading paths have been used by several investigators to investigate the stresses arisen from the strain-path. The purpose of these experiments was to determine the relationship between stress components and the given plastic strain increment and was not related to the determination of yield surface. These experiments will be discussed in Section 7.5. 7.2.3

Yield Surface Versus Loading Surface

Based on experimental observations, Phillips and his coworkers proposed the idea of loading surface. A description of two-surface theory may be found in

© 2005 by Chapman & Hall/CRC Press

334

Continuum Mechanics and Plasticity 3

C

A b a

O II

I c

III

B d D

FIGURE 7.7 Motion of yield surface and the loading surface (From Phillips, A., Int. J. Plasticity, 2, 315, 1986. With permission from Elsevier).

Phillips [27]. The main concept that is different from the traditional concept of plasticity is to consider plastic ﬂow as rate dependent. Plastic strain takes time to develop and the existence of an equilibrium stress is postulated at which plastic strain is fully developed, see Wu [28], Phillips and Wu [29], Phillips [30], and Krempl [31]. A loading surface represents the largest state of stress achieved in the loading history, and it expands isotropically upon loading. Figure 7.7 shows the motion of the yield surface and the loading surface in the stress space. The yield surface tends to become tangential to the loading surface when it moves towards the loading surface. But, when the stressing point penetrates the loading surface, it will drag the loading surface with it and the loading surface expands. Referring to Figure 7.7, the initial yield surface which is also the initial loading surface is denoted by I. A stress path from O to A will cause the loading surface to expand to the surface labeled as II, and a stress path AD will cause the loading surface to expand further to Surface III. On the other hand, stress path AC does not cause the loading surface to expand because path AC does not penetrate the corresponding loading surface, Surface II. Surfaces labeled as a, b, c, and d are yield surfaces. Since plastic strain takes time to develop, the experimentally determined yield surface after path OA is Surface a only after the stressing point has stayed at A for a sufﬁcient length of time. If the prestress point does not stay at A for a sufﬁcient length of time before the yield surface is probed, then the obtained yield surface will

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

335 T T1

Troom

3

FIGURE 7.8 Yield Surface in the stress–temperature space (From Phillips, A., Int. J. Plasticity, 2, 315, 1986. With permission from Elsevier).

be a distance away from the loading surface and does not touch the loading surface. 7.2.4

Yield Surface at Elevated Temperature

Phillips and his coworkers [32–35] conducted a series of experiments and determined yield surfaces at elevated temperatures which were lower than 0.3Tm , where Tm is the absolute melting temperature of the material. Thinwalled tubes of 1100-0 aluminum were tested. The yield surface in the stress–temperature space is shown schematically in Figure 7.8, where the surface is depicted between two constant temperatures T1 and Troom with T1 > Troom . An isothermal yield surface may be obtained by passing a plane normal to the temperature axis. The yield surface (the isotherm) shrinks as the temperature increases. The yield surface is actually a conoid with a ridge at the top. The length of the ridge depends on the prestrain history, measured by equivalent plastic strain. The initial yield surface is a cone with an elliptical base. The length of the ridge is zero because the equivalent plastic strain is zero. As the equivalent plastic strain increases with the prestraining history, the length of the ridge also increases with a narrower width for the corresponding isothermal yield surfaces. A ridge is formed when the width of the isothermal yield surface at the top is zero. The ridge is perpendicular to the direction of preloading. For each value of equivalent plastic strain, there corresponds a temperature Tmax which deﬁnes the height of the conoid with a ridge at the top. The temperature Tmax decreases with the increasing equivalent plastic strain. Finally, we mention that the distortion and motion of the yield surface can occur either by an increment of loading history or by a temperature increment or by a combination of the two. Figure 7.9 shows a case of initial and subsequent isothermal yield surfaces determined by Phillips and Tang [22] at 21, 66, 108, and 152◦ C (70, 151, 227, and 305◦ F) due to prestress in tension.

© 2005 by Chapman & Hall/CRC Press

336

Continuum Mechanics and Plasticity

2.0

6 A⬘ 10 22

1.0

227

30

Shear Stress (KSI)

26

0

3 28 227°F

14 18

°F

5°F

27 23 19 75 8 17 21 25 29

305°F

–1.0

Specimen S–5

70°F 151 °F

13 16

9 12

24

20

151°F 15

70°F 7 A⬘

2×

4

A

First Sub Yield Surface Prestressing at A 2 = 5507 lb/in T = 70°F p = 45 µ⬙/u

11

Initial Yield Surface –2.0 0

1.0

2.0

3.0

4.0

5.0

6.0

Tensile Stress (KSI)

FIGURE 7.9 A case of initial and subsequent isothermal yield surfaces (From Phillips, A. and Tang, J.L., Int. J. Solids Struct., 8, 463, 1972. With permission from Elsevier).

7.3

The Direction of the Plastic Strain Increment

It was mentioned in Section 6.3 that an important assumption concerning p the plastic strain increment dεij is that the principal axes of plastic strain increment and deviatoric stress are coincident, which is known as the norp mality rule and which says that dεij is normal to the yield surface. It was also mentioned that this assumption has been experimentally veriﬁed. But, it is to be emphasized here that those veriﬁcations were valid for initial yield surface p only. The following question remains: Is dεij normal to the subsequent yield surface? A direct answer can be found from the works of Phillips and Moon [14] and Ohashi et al. [36] who showed that the plastic strain increment is indeed normal to the subsequent yield surfaces. Figure 4 of Phillips and Moon [14] is reproduced as Figure 7.10. In the ﬁgure, the initial yield surface is labeled as 0 and the ﬁrst prestressing path is OA. The yield surface corresponding to A is labeled as I. In this discussion, we do not emphasize the difference between a loading surface and a yield surface as the writers did. The next stage of stressing went from B to C in tension. Path BC is nearly tangential to the ﬁrst subsequent yield Surface I. The second subsequent yield surface labeled as II was then determined. This surface

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

337

4

3

A I

2

II B

C

× 10–3 psi

1 III 0 0

D

3

4

5

6 × 10–3 psi

7

–1 IV –2 E –3

–4

Specimen M-3

FIGURE 7.10 Plastic strain increment vector (From Phillips, A. and Moon, H., Acta Mech., 27, 91, 1977. With permission from Springer).

shows further distortion from the previous surface and it translated not only in the direction of prestressing but also by a small amount in the direction perpendicular to the prestressing direction. Owing to the distortion, it is difﬁcult to judge whether rotation had taken place in yield Surface II. The directions p of dεij along path BC are also shown in the ﬁgure. These directions rotated from the direction normal to the yield surface from which the prestressing was initiated to the direction normal to the ﬁnal yield surface. We note that this stress path is similar to tor–ten path (5) discussed in Section 7.2.2.2. The second stage of both paths is tangential to the yield surface. The only difference is that the path of Phillips and Moon started from the opposite side of the ﬁrst subsequent yield surface, while path (5) starts from the prestress point A. Another stress, similar in nature, is shown in Figure 7.10. Starting from the yield surface labeled as III, stress path DE was applied. This stress path was again nearly tangential to the yield surface. At the end of the stressing, a yield surface was determined and labeled as IV. A distortion of yield surface had taken place and the surface had moved not only in the direction of prestressing but also in the lateral direction. Owing to the distortion, it is difﬁcult to judge whether the yield surface had rotated. Small vectors in the p ﬁgure show the variations in the direction of dεij .

© 2005 by Chapman & Hall/CRC Press

338

Continuum Mechanics and Plasticity 3 – 139°

131°

120° 107°

150°

100° 90°

1.0

B 164°

60° A

0.5

30° I = 4 3 2 1 0.5 0.2 0.1 0.05 180°

0.02% 0°

–10

–0.5

0

0.5

1.0

–

z/

FIGURE 7.11 Plastic strain increment vector (From Ohasi, Y. et al., J. Mech. Phys. Solids, 23, 277, 1975. With permission from Elsevier).

Ohashi et al. [36] prestressed a tubular specimen in tension (ﬁrst stress path) to a tensile stress of σz /σ¯ = 1.0, where σ¯ = 235 MPa. The corresponding prestrain at this point was 2%. A second stress path was then applied in combined axial–torsion, emanating from the prestress point making an angle θ with the ﬁrst stress path. Figure 3 of Ohashi et al. [36] is shown as Figure 7.11, in which θ = 0, 30, 60, 90, 100, 107, 120, 131, 139, 150, 164, and 180◦ . The strain data along each stress were recorded and the equi-strain curves √ path p 2 p 2 1/2 based on Iε = {(ε ) + (γ / 3) } and corresponding to Iε = 0.02%, 0.05%, 0.1%, 0.2%, 0.5%, and 1%, 2%, 3%, and 4% are found and shown in the ﬁgure. These curves are similar to subsequent yield surfaces determined by the use of different amounts of proof strains, and these are yield surfaces corresponding to the prestress point at σz /σ¯ = 1.0. The short segments on the second stress path√for each θ show the directions of the plastic strain increment vector (γ p / 3, εp ). Ohashi et al. [36] found that the plastic strain increment vector is almost normal to the equi-strain curves, except for the range of Iε ≤ 0.05% and 139◦ < θ < 164◦ . Other investigations of the plastic strain increment did not report the yield surfaces along the stress paths and therefore the information provided is not complete enough to directly beneﬁt the constitutive modeling. Nevertheless, these works are useful in that they can provide qualitative results for certain observed behaviors of materials. Phillips and Kaechele [37] conducted stresscontrolled tests on thin-walled tubes of aluminum 2S-O following tor–ten path (5) and ten–tor path (7). The tests were conducted in a strain range √ up to 1.5%. The stress paths are shown schematically in Figure 7.12 in the ( 3τ , σ ) space. The short segments on the √ stress paths show the directions of the plastic strain increment vector (γ p / 3, εp ). For tor–ten path (5), the plastic strain increment was along the shear direction before a sudden change of direction

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

339 3

O

FIGURE 7.12 Plastic strain increment vector (From Phillips, A. and Kaechele, L., J. Appl. Mech., 23, 43, 1956).

3 D

C F

E

O

B

A

FIGURE 7.13 Stress paths of Khan and Wang (From Khan, A.S. and Wang, X., J. Mech. Phys. Solids, 36, 519, 1988. With permission).

took place in the stress path. The direction of the plastic strain increment gradually changes afterward. In the case of ten–tor path (7), the plastic strain increment was initially along the tension direction and the direction gradually changes after the change in direction of the stress path. Khan and Wang [38] conducted combined axial–torsion tests on OHFC copper, following two stress paths shown in Figure 7.13. In path OABC, the specimen was ﬁrst stressed in tension to A into the plastic region. Partial unloading and reverse loading then took place from A to B while keeping the shear stress zero. Finally, torsion was increased from B to C while keeping the axial stress constant. In path ODEF, the specimen was subjected to shear stress from O to D, unloading from D to E, and then loading from E to F. The two paths are similar in nature. The corresponding strain paths are shown schematically in Figure 7.14. From the ﬁgure we see that during segment BC of path OABC, the increment of axial strain ε changes from negative to positive as the shear stress increases while keeping the axial stress σ constant. Similarly, during segment EF of path ODEF, the increment of shear strain γ changes from negative to positive as the axial stress increases while keeping

© 2005 by Chapman & Hall/CRC Press

340

Continuum Mechanics and Plasticity 3

E

F C

O

B

FIGURE 7.14 The corresponding strain paths of Khan and Wang (From Khan, A.S. and Wang, X., J. Mech. Phys. Solids, 36, 519, 1988. With permission).

the shear stress τ constant. The curves have been exaggerated to show the sign change in dε and dγ .

7.4

Multisurface Models of Flow Plasticity

It was mentioned in Section 7.2.3 that Phillips [27] proposed a multisurface model in which the yield surfaces are bounded by the loading surface. However, in most of the investigations by Phillips, emphasis was placed on how to describe the change of the yield surface and the direction of the plastic strain increment. Little was done to propose and verify the ﬂow rule in terms of plastic modulus, particularly for complex loading paths including unloading and reloading. With a correctly determined plastic modulus, the ﬂow rule should describe the nonlinear stress–strain curves. Multisurface models that attempt to accomplish just that are discussed in this section. These models emphasize the description of cyclic loading behavior. 7.4.1

The Mroz Kinematic-Hardening Model

The work of Mroz [39] has a large following, particularly in computational mechanics. Mroz approximated the one-dimensional stress–strain curve OABCDE by n linear segments of constant tangent moduli E1 , E2 , . . . , En , as in Figure 7.15. The tangent modulus decreases as the strain increases. This is the idea of a “ﬁeld of work-hardening moduli.” If the stress–strain curve of Figure 7.15 is projected onto the stress space, then we have a one-dimensional stress space in the σ -axis. In the multidimensional stress space, this ﬁeld is deﬁned by a conﬁguration of surfaces of constant work-hardening modulus. Each nodal stress (stress at A, B, C, etc.) is represented by a surface

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

341

E

E9 E8

E6

E7

C5

C4

B3

C

B

D

A

O B1 B2

C3 E5

C2

C1

E1

E2

E3

E4

FIGURE 7.15 Mroz’s Field of work-hardening moduli concept.

geometrically similar to the initial yield surface but of different size. These surfaces are expressed by (m) 2 fm σij − αij = Ym

(7.2)

where m = 0, 1, 2, …. Using the Mises yield criterion, the surfaces are concentric circles in the two-dimensional stress space, as shown in Figure 7.16(a). Thus, surface fA is the initial yield surface passing through point A of Figure 7.15 and fB is the surface passing through point B, etc. In Mroz’s hardening rule, the surfaces cannot intersect but consecutively contact at similar points and push each other. Similar points are stress points on different surfaces with the same outward normal. During loading sequence OABCDE, surface fA translates so as to touch surface fB at the point of loading; next, surfaces fA and fB move together until they contact surface fC , and so on. The surfaces at stress state C are shown in Figure 7.16(b). Since all surfaces can contact only at the similar points, the active surface translates in the direction parallel to the vector connecting the current stress point σm to the corresponding similar point σm+1 of the next surface. This hardening rule is expressed by dαm = dµ (σm+1 − σm )

(7.3)

where dµ is a scalar to be determined by the consistency condition; dαm describes the translation of the active surface fm . Figure 7.17 is a sketch of Mroz’s hardening rule.

© 2005 by Chapman & Hall/CRC Press

342

Continuum Mechanics and Plasticity 2

(a)

E D C B A

fC fD

fA

(b)

E

1

fB

O

fE

(c) C

D C

C5

fE fD

C4

fC fB

fA fB C1 C2 C3

fC

fA fD

fE C3

FIGURE 7.16 (a) A family of concentric circles, (b) surfaces at stress state C of Figure 7.15, (c) surfaces at stress state C3 of Figure 7.15.

The discussion of the one-dimensional loading shown in Figure 7.15 is continued here. After reaching stress state C shown in Figure 7.16(b), if unloading takes place, then the stress point will move from C to C1 elastically. Reverse plastic ﬂow occurs at C1 and surface fA translates downwards until it contacts surface fB at C2 . We see from the ﬁgure that the stress difference between C1 and C2 is twice that between A and B. Further unloading from C2 to C3 will induce additional plastic deformation and the stress point carries surfaces fA and fB with it until it contacts surface fC at C3 . This state of stress is shown in Figure 7.16(c). We mention again that the stress difference between C2 and C3 is twice that between B and C. The reloading from C3 to C4 is again elastic, but plastic deformation occurs from C4 to C5 . The stress point carries surface fA with it until it contacts surface fB . Further loading from C5 to C translates both

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

343 m + 1

m d

m

m + 1 fm

fm + 1

Stress Space FIGURE 7.17 Mroz’s hardening rule.

C n P

R

n

Q

S n T

fA fB fC FIGURE 7.18 A case of nonproportional loading (Mroz’s model).

fA and fB and returns the stress state back to C, as shown in Figure 7.16(b). We have thus completed one cycle of loading–unloading–reloading. Additional loading cycles follow the same path C–C1 –C2 –C3 –C4 –C5 –C and this is the steady loop and no cyclic hardening is possible by use of Mroz’s model. We also show in Figure 7.15 a steady loop with unloading starting at B and a loop with unloading starting at E. Looking at a loop of cyclic loading, we ﬁnd that the difference in stress for each piecewise-linear step during unloading or reloading is twice that of the corresponding step during loading. The difference in the strain for each step also has the same characteristic. We may conclude that the slopes of E1 E2 and E6 E7 are the same as that of AB, and the slopes of E2 E3 and E7 E8 are the same as that of BC, etc. In fact, the loading, unloading, and reloading curves are similar and they satisfy Masing’s formula [40]. A case of nonproportional loading is now considered. Upon loading to C as in Figure 7.16(b), the specimen is partially unloaded to a point P, Figure 7.18.

© 2005 by Chapman & Hall/CRC Press

344

Continuum Mechanics and Plasticity

The stress point then moves along PQ, and when it reaches point R, it will move along the direction of RS. The normal to surface fB at S is the same as the normal to surface fA at point R. S is the point at which fA will be tangential to and not intersecting fB . In the next step the stress point will move from S to T. Again, the normal to fC at T is parallel to the normal previously mentioned at R and S. The work-hardening modulus on this loading path decreases and becomes equal to that at C when the stress path intersects fC at T. Mroz [39] used this example to illustrate a case of nonproportional loading. We remark that the stress path after the partial unloading is PRST and not PRQ. In a stresscontrolled tor–ten test, with stress point moving along PQ as in paths (4) and (5) of Figure 7.2, the contact between fA and fB takes place at a location other than S. 7.4.2

The Two-Surface Model of Dafalias and Popov

Dafalias and Popov [41,42] proposed a two-surface model and deﬁned a continuous variation of the plastic modulus dσ/dε p = Ep between these two surfaces. This is in contrast to Mroz’s model presented in Section 7.4.1, which proposes a piecewise constant plastic moduli ﬁeld and a number n of associated surfaces. In the two-surface model a bounding surface is proposed in the stress space in addition to the yield surface (sometimes also called the loading surface). The loading surface is used interchangeably with the yield surface in this discussion and does not have the same meaning as that deﬁned by Phillips, mentioned in Section 7.2.3. The bounding surface always encloses the yield surface and is a generalization of the bounds observed in the experimental results for uniaxial random cyclic loading on a grade 60 steel specimen. The details of the experimental random cyclic loading curve were presented in [41]. Figure 7.19 shows a simpliﬁed schematic cyclic curve with some parameters of the model indicated. Lines XX and YY are the bounds for the material tested. They can be curves for other materials. Curve 0–1–2 is a loading stress–plastic strain curve and it merges with the bounding line XX when the loading continues. If unloading occurs at point 2, then the unloading curve would follow 2–3–4 and merge with the bound line YY . On the other hand, if reloading starts at A, then AB is elastic and plastic deformation begins to occur at B. Experimental results indicated that the curve after B is steeper than curve Section 3–A, that is, the plastic moduli are not of the same magnitude between the two curve sections. Dafalias and Popov [41,42] suggested that Ep be a function of two parameters, the distance δ of the stress state under con¯ and the value sideration, such as point A, from the corresponding bound A, of δ at the initiation of yielding for each loading process, denoted by δin . The δin changes at each reversal and is associated with the most recent event of unloading–reloading. In fact, this is an assumption of fading memory, where the material remembers only the most recent loading history. Thus, we write Ep = Ep (δ, δin )

© 2005 by Chapman & Hall/CRC Press

(7.4)

Advances in Plasticity

345 2

B

b

X⬘

b

X

B

1

3

O

p

in A

a a Y⬘

Y

A

4

FIGURE 7.19 Bounds and parameters of two-surface model.

with the property that Ep → ∞

when δ → δin

(7.5)

for a smooth transition from the elastic into elasto-plastic range and E¯ p = Ep (0, δin )

when δ → 0

(7.6)

where E¯ p is the slope of the bound line and Ep monotonically increases as δ decreases. Dafalias and Popov [42] recommended the following expression for Ep : δ Ep = E¯ p + h (7.7) δin − δ where h is a function of δin and a nonlinear form for h has been chosen to model the complex random cyclic loading curve presented in Dafalias and Popov [41]. ¯ and B¯ are projected onto the Referring to Figure 7.19 again, points A, B, A, ¯ a and stress axis and the corresponding points are denoted by a, b, a¯ , and b. b are points on the yield surface, whereas a¯ and b¯ are points on the bounding surface. The rates of change of centers of yield and bounding surfaces are related to the plastic strain rate by α˙ = Eα ε˙ p

© 2005 by Chapman & Hall/CRC Press

(7.8)

346

Continuum Mechanics and Plasticity

and β˙ = Eβ ε˙ p = α˙ − (Eα − Eβ )˙ε p

(7.9)

respectively. When there is no isotropic hardening of the yield surface, Eα = Ep ; and when there is no isotropic hardening of the bounding surface, Eβ = Ep . In this case, the two bounds are parallel straight lines in the one-dimensional case. In the multiaxial stress space, the yield surface f and the bounding surface f¯ are f (σij − αij , qn ) = 0

and

f¯(σ¯ ij − βij , qn ) = 0

(7.10)

where αij and βij denote the centers of f and f¯, respectively, and qn are internal variables (which will be further discussed in Chapter 8). The two surfaces may deform and translate in stress space in a coupled way. The evolution of qn is given by q˙ n = q˙ n (σij , σ˙ ij , qm , ξm )H(L)

when f = 0

q˙ n = 0

when f < 0

(7.11)

where H(L) is the Heaviside step function and L is the loading function, which under the isothermal condition is L = σ˙ = σ˙ ij nij

(7.12)

in which n is the unit normal to the yield surface. Internal variables qn represent the dependence of the yield surface on the history of deformation. One of the qn may describe isotropic hardening. ξm in (7.11) are internal variables associated with abrupt changes of the loading processes. In the present case, they are the δin ’s. These parameters remain constant during the loading process. The continuously changing δ and the initial value δin deﬁne the generalized plastic modulus K with the properties K = K(δ, δin ),

K¯ = K(0, δin ),

K(δin , δin ) = ∞

(7.13)

where K¯ is the generalized plastic modulus on the bounding surface and is an increasing function of δ for a given δin . The distance δ is from point a on the yield surface f = 0 to a similar point a¯ on the bounding surface f¯ = 0 (see Figure 7.20). At similar points, the normals to the respective surfaces are equal. Let the stress at point a be σij and the stress at point a¯ be σ¯ ij , then δ is deﬁned by δ = [(σ¯ ij − σij )(σ¯ ij − σij )]1/2

© 2005 by Chapman & Hall/CRC Press

(7.14)

Advances in Plasticity

347 22

a

ij ij a

Yi e l d

ac

ij

e

ij

nij

Su

rf

11

O u rf gS B o undi n

ac e

FIGURE 7.20 Two-surface model in two-dimensional stress space (From Dafalias, Y.F. and Popov, E.P., J. Appl. Mech., 98, 645, 1976. With permission from ASME).

For simplicity, we assume that the bounding surface is an isotropic expansion of f = 0, but both surfaces are allowed to move. The centers for the two surfaces are αij and βij , respectively, as shown in Figure 7.20. Since the two surfaces are similar, the radii connecting the two centers and the corresponding stress points are parallel. Thus, it is written as σ¯ ij − βij = m(σij − αij )

(7.15)

where m is a proportional factor which can be a function of qn . This relation may be further written as σ¯ ij − σij = m(σij − αij ) + βij − σij

(7.16)

and be substituted into (7.14) to obtain an expression for δ. Several rules of evolution of αij and βij have been used in the literature in conjunction with the two-surface model. The following discussion follows p Dafalias and Popov [42]. Assuming linear dependence of ε˙ ij on the stress rate, the ﬂow rule, assuming normality, is p

ε˙ ij =

1 Lnij K

(7.17)

where is the Macauley bracket deﬁning the operation L = LH(L). From (7.17), we found p p 1/2 L = σ˙ = K ε˙ ij ε˙ ij

© 2005 by Chapman & Hall/CRC Press

(7.18)

348

Continuum Mechanics and Plasticity

Working with the magnitudes and projection of the stress rate onto the normal direction, this relation is a generalized relation of σ˙ = Ep ε˙ p in the onedimensional case, that is, Ep has been generalized into K. We now use the same procedure to generalize (7.8) by writing p p 1/2 Kα α˙ = α˙ ij nij = K α ε˙ ij ε˙ ij L = K

(7.19)

Denoting the unit vector along α˙ ij by νij , which is, in general, not in the same direction as nij , we may write α˙ ij = α˙ ν νij

(7.20)

where α˙ ν is the magnitude. Substituting (7.20) into (7.19), we have α˙ = α˙ ij nij = α˙ ν νij nij

(7.21)

α˙ 1 Kα νij = Lνij νrs nrs νrs nrs K

(7.22)

Therefore, α˙ ij =

The modulus K α /K can be determined by substituting (7.22) into the consistency condition. Referring to the yield surface given in (7.10), the consistency condition is ∂f ∂f ∂f f˙ = q˙ n = 0 σ˙ ij + α˙ ij + ∂σij ∂αij ∂qn

(7.23)

Denoting the magnitude of ∂f /∂σij by g=

∂f ∂f ∂σij ∂σij

1/2 (7.24)

we write ∂f = gnij ∂σij

(7.25)

In addition, we assume that q˙ n is linear in σ˙ ij , that is, q˙ n = rn L

(7.26)

where rn is a scalar. Using (7.24) to (7.26), (7.23) reduces to Kα 1 ∂f rn =1+ K g ∂qn

© 2005 by Chapman & Hall/CRC Press

(7.27)

Advances in Plasticity

349

We then substitute (7.27) into (7.22) to obtain α˙ ij . This relation applies to any kinematic-hardening rule for which νij is speciﬁed. A special case is obtained when ∂f /∂qn = 0. In this case, K α = K, which corresponds to Eα = Ep in the one-dimensional case. The same procedure may be used again to generalize (7.9). By differentiating (7.10), the consistency condition for the bounding surface is ∂ f¯ ˙ ∂ f¯ ∂f f˙¯ = σ¯ ij + β˙ij + q˙ n = 0 ∂ σ¯ ij ∂βij ∂qn

(7.28)

Writing

∂ f¯ ∂ f¯ ∂ σ¯ ij ∂ σ¯ ij

1/2

∂ f¯ = g¯ nij ∂ σ¯ ij

(7.29)

p p 1/2 K¯ L¯ = σ˙¯ = σ˙¯ ij nij = K¯ ε˙ ij ε˙ ij = L K

(7.30)

g¯ =

,

and

and using them in (7.28), the consistency condition is nij β˙ij = L¯ +

1 ∂ f¯ rn L g¯ ∂qn

(7.31)

We now generalize (7.9) to obtain p p 1/2 Kβ β˙ = β˙ij nij = K β ε˙ ij ε˙ ij = L K

(7.32)

and denote the unit vector along β˙ij by ξij , then β˙ij = β˙ ξ ξij

(7.33)

where β˙ ξ is the magnitude. But, β˙ is the projection of β˙ij along nij , and, therefore, we have β˙ = β˙ij nij = β˙ ξ ξij nij

and

β˙ ξ =

β˙ ξij nij

(7.34)

Hence, β˙ij =

© 2005 by Chapman & Hall/CRC Press

β˙ 1 Kβ ξij = Lξij ξrs nrs ξrs nrs K

(7.35)

350

Continuum Mechanics and Plasticity

For simplicity, consider a case νij = ξij = µij . This assumption is similar to Mroz’s hardening rule, where µij is a unit vector going from point a to point a¯ (see Figure 7.20). For this case, (7.22) reduces to α˙ ij =

1 Kα Lµij µrs nrs K

(7.36)

β˙ij =

1 Kβ Lµij µrs nrs K

(7.37)

and (7.35) reduces to

Analogous to the second expression of (7.9), we write β˙ij = α˙ ij − Mµij

(7.38)

From (7.36) to (7.38), the following is obtained M=

1 Kα − Kβ L µrs nrs K

(7.39)

Substituting (7.30), (7.38), and (7.39) into (7.31) obtains Kβ K¯ 1 ∂ f¯ = + rn K K g¯ ∂qn

(7.40)

Using (7.27) and (7.40), (7.39) may be further written as 1 M= µrs nrs

K¯ 1− K

+

1 ∂ f¯ 1 ∂f rn − rn g¯ ∂qn g ∂qn

L

(7.41)

In the case that both f and f¯ are not functions of qn , (7.41) becomes 1 M= µrs nrs

K¯ 1− K

L

(7.42)

¯ In the limit, when the yield surface contacts the and (7.40) yields K β = K. ¯ the two surfaces will then move together bounding surface, δ = 0, and K = K, upon further loading. From (7.36) and (7.37), we have β˙ij = α˙ ij

© 2005 by Chapman & Hall/CRC Press

(7.43)

Advances in Plasticity

7.5

351

The Plastic Strain Trajectory Approach

The strain (total strain, not plastic strain) trajectory approach was initiated by Ilyushin [43,44], who represented the stress and deviatoric strain tensors in a ﬁve-dimensional vector space. He then investigated the characteristics of the stress response to a predetermined strain trajectory. Further investigations using this approach are reported by Lensky [45] and Ohashi and his coworkers [3,36,46,47]. A theory by Pipkin and Rivlin [48] is similar to Ilyushin’s theory but using strain tensors, and Zhou et al. [49] consider the plastic strain trajectory. In an independent effort, Valanis [1,2] developed an endochronic theory of plasticity using irreversible thermodynamics of internal variables. The resulting constitutive equation, if expressed in an integral form, resembles that presented by Ilyushin [50]. In this constitutive equation, stress is a functional of the plastic strain history. The differences between the two developments will be addressed in Section 7.5.2. Wu and his coworkers [51–55] have contributed to the experimental veriﬁcations and applications of the endochronic theory. The endochronic theory of plasticity will be further discussed in Chapters 8 and 9. 7.5.1

The Theory of Ilyushin

Ilyushin worked with the deviator of the strain tensor (not plastic strain). When the strain is large, the plastic strain may be approximated by the total strain. The theory is, however, not suitable for describing the elastic–plastic transition behavior. The deviatoric strain eij has only ﬁve independent components. Thus, eij may be represented by a vector in a ﬁve-dimensional space as e=

5

ε i ui

(7.44)

i=1

in which ui are unit vectors along axes of the ﬁve-dimensional space. The magnitude of this vector must be equal to the magnitude of tensor eij , so that

eij eij ≡

i,j=1,2,3

If we deﬁne ε3 =

√ 2e12 ,

ε4 =

5

(εi )2

(7.45)

i=1

√ 2e23 ,

ε5 =

√ 2e31

(7.46)

then (7.45) and (7.46) are reduced to (e11 )2 + (e22 )2 + (e33 )2 = (ε1 )2 + (ε2 )2

© 2005 by Chapman & Hall/CRC Press

(7.47)

352

Continuum Mechanics and Plasticity 2⬘

6

2

3⬘

6 +

6

– 6

1⬘ 2 – 3

1

FIGURE 7.21 Coordinate transformation in the deviatoric strain plane.

The relationships between components of (ε1 , ε2 ) and (e11 , e22 ) are found from the coordinate transformation given in Figure 7.21. Note that e33 = −(e11 + e22 ). In the ﬁgure, axes 1 , 2 , and 3 denote the coordinate axes for e11 , e22 , and e33 , respectively, in the π -plane; whereas 1 and 2 denote the axes of ε1 and ε2 . The 1-axis is making angle β with the 1 -axis. Projecting ε1 and ε2 onto the 1 and 2 directions, respectively gives

e22

e11 = m(ε1 cos β + ε2 sin β)

π π = m −ε1 sin β + + ε2 cos β + 6 6

(7.48a) (7.48b)

where the factor m is introduced √so that (7.47) is satisﬁed. Substituting (7.48) into (7.47), we obtain m = 2/3. Using this value of m, we found from (7.48) that 3 = ε1 cos β + ε2 sin β e11 2

3 π π (7.49) e22 = −ε1 sin β + + ε2 cos β + 2 6 6

3 π π e33 = ε1 sin β − − ε2 cos β − 2 6 6 The third equation of (7.49) was found from e33 = −(e11 + e22 ). The ﬁrst two equations of (7.49) may then be solved to obtain

√

π − e22 sin β ε1 = 2 e11 cos β + 6 (7.50)

√

π ε2 = 2 e11 sin β + + e22 cos β 6

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

353

Finally, if the angle is set to β = 0, then we have ε1 =

√ 1 ε2 = 2 e22 + e11 , 2 √ √ ε4 = 2e23 , ε5 = 2e31

3 e11 , 2

√ ε3 = 2e12 ,

(7.51)

These are the ﬁve components in the plastic strain space.

+σ +σ = 0 may be represented Similarly, the deviatoric stress σij with σ11 22 33 in a ﬁve-dimensional stress space by the following components: σ1 =

√ 1

σ2 = 2 σ22 + σ11 , 2 √

√

σ4 = 2σ23 , σ5 = 2σ31

3

σ , 2 11

√

σ3 = 2σ12 ,

(7.52)

The next step is to establish a relationship between the stress and the strain increment, and this relationship is expressed in terms of the arc length s measured along the strain path. In the case of combined axial–torsion, the stress is (σ1 , σ3 ) and the strain increment is (dε1 , dε3 ). A plane strain trajectory is shown in Figure 7.22, and the arc length is ds =

(ε1 )2 + (ε3 )2

(7.53)

If the current strain state is represented by point A, unit vector p1 is tangential to the trajectory at A, and unit vector p3 is the principal normal. A similar ﬁgure is presented in [49] but in the plastic strain space. According to the Frenet formulas for curves in space, we have the following relations: dp3 = −κp1 ds

dp1 = κp3 , ds 3

p3

(7.54)

e3 A

p1 e1

Str ain

tr

e aj

ry cto

O

1

FIGURE 7.22 A plane strain trajectory and stress (From Zhou, Z.-D. et al., Int. J. Plasticity, 19, 1377, 2003. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

354

Continuum Mechanics and Plasticity

where κ is the curvature. Writing the stress vector as σ = Pp1 + Np3

(7.55)

Lensky [45] and Ohashi and his coworkers [3,36,46,47] conducted combined axial–torsion experiments to determine the variations of P, N, the magnitude of σ, denoted by σ , and the angle of delay θ between vectors σ and dε as functions of s. The angle of delay is found from cos θ =

σ · dε σ ds

(7.56)

These authors believe that these relationships are the constitutive equations of the material under investigation. Trajectories investigated include proportional strain trajectories, strain trajectories with two straight branches, orthogonal bilinear trajectories with a rounded corner, and more general curvilinear strain trajectories. The results show that the arc length s and the curvature κ are two important parameters deﬁning the constitutive behavior of the material. Ilyushin proposed a postulate of isotropy, see [45], which states that, for a strain trajectory starting from the origin of the strain space, the stress response is deﬁned by the intrinsic geometry of the strain trajectory and is invariant with respect to transformation of strain trajectory by means of rotation or reﬂection. Ilyushin further proposed the principle of delay, which states that the stress response to a strain trajectory is not deﬁned by the whole strain trajectory, but by the recent past of the trajectory with length λ known as the trace of delay. This is in fact a statement of fading memory. In the case of a curved trajectory followed by a straight trajectory, at a distance λ after the beginning of the straight trajectory, the stress vector becomes tangent to the trajectory. This is a very intuitive statement, because experimental results show that the stress path and the strain path do not coincide even for a proportional straining. Ilyushin [50] further proposed the following integral constitutive equation σ(s) =

0

s

K[s, s ; κi (s), κi (s )]dε(s ),

i = 1, 2, 3, 4

(7.57)

where s is the running parameter of integration; the kernel function multiplied by dε(s ) represents the contribution of dε(s ) to the stress vector at s ; and κi represents the geometry of the strain trajectory. A recent derivation of (7.57) by Zhou et al. [49] in the plastic strain space is now discussed with permission from Elsevier. p p Referring to Figure 7.22, in which the axes should be renamed ε1 and ε3 , the plastic strain increment is p

p

dεp = dε1 e1 + dε3 e3 = dsp1

© 2005 by Chapman & Hall/CRC Press

(7.58)

Advances in Plasticity

355

and the stress is σ = σ1 e1 + σ3 e3 = σ (cos θ p1 + sin θp3 )

(7.59)

where ei are base vectors of the Cartesian coordinate system; and θ is the angle of delay between vectors σ and dεp . We now deﬁne the length of the plastic strain path by ds =

p 2 p 2 ε1 + ε3

(7.60)

Differentiating (7.59) with respect to s and using (7.54), we obtain σ˙ = g1 p1 + g3 p3

(7.61)

where g1 = σ˙ cos θ − σ (κ + θ˙ ) sin θ ,

˙ cos θ g3 = σ˙ sin θ + σ (κ + θ)

(7.62)

We now make use of the transformation equations p1 = cos ηe1 + sin ηe3 ,

p3 = − sin ηe1 + cos ηe3

(7.63)

and the relations p

cos η =

p

dε1 , ds

sin η =

dε3 ds

(7.64)

and substituting (7.63) and (7.64) into (7.61) to obtain

p

p

dε dε σ˙ = σ˙ 1 e1 + σ˙ 3 e3 = g1 1 − g3 3 ds ds

p

p

dε dε e1 + g1 3 + g3 1 ds ds

e3

(7.65)

We have thus found from (7.65) that g dσ1 = 1 dσ3 g3

−g3 g1

p

dε1

p

dε3

(7.66)

Experimental results show that σ can be expressed by σ (s − s , κ) =

n Rρ −Aρ (s−s ) e , Aρ

ρ=1

© 2005 by Chapman & Hall/CRC Press

Aρ = Aρ (s, κ)

(7.67)

356

Continuum Mechanics and Plasticity

where Rρ and Aρ are material constants. Substituting (7.67) into (7.62) and neglecting terms of higher order of smallness, we obtain g1 =

3

Rρ Nρ e−Aρ (s−s ) ,

Nρ = cos θ − sin θ

ρ=1

g3 =

3

(κ + (dθ/ds)) Aρ (7.68)

Rρ Mρ e−Aρ

(s−s )

(κ + (dθ/ds)) Mρ = sin θ + cos θ Aρ

,

ρ=1

Substituting (7.68) into (7.66) and integrating the equation, yields 3 s σ1 −Aρ (s−s ) Nρ = Rρ e σ2 Mρ 0 ρ=1

−Mρ Nρ

p

dε1

p

dε3

(7.69)

This is the constitutive equation for a plastic strain trajectory. 7.5.2

The Endochronic Theory of Plasticity

The endochronic theory of plasticity was developed by Valanis [1] from the thermo-mechanical theory of internal variables. The theory will be discussed in detail in Chapter 8. The word endochronic is a Greek word for intrinsic time or internal time. Valanis introduced an intrinsic time ζ , which is monotonically increasing and is deﬁned by dζ 2 = Pijkm dεij dεkm

(7.70)

where Pijkm is a positive deﬁnite material tensor. In a special case, dζ may be deﬁned by the length of the strain path, that is, dζ 2 = dεij dεij

(7.71)

The constitutive equation has two parts, the deviatoric and volumetric part. They are σij

=2

ζ

ζ0

σkk = 3

ζ

ζ0

µ(ζ − ζ )

deij

dζ dζ

dεkk K(ζ − ζ ) dζ dζ

(7.72)

where µ(ζ ) and K(ζ ) are kernels of the integrals. In the one-dimensional stressing, (7.72) reduces to σ =

© 2005 by Chapman & Hall/CRC Press

ζ 0

E(ζ − ζ )

dε dζ

dζ

(7.73)

Advances in Plasticity

357

where E(ζ ) is a kernel function. Equations (7.72) and (7.73) are in the same form as (7.57), except that only the length of the strain path and not the curvature nor the torsion of the strain trajectory is included in the formulation. These geometrical parameters of the strain path may be accounted for by use of internal variables, and they have not been included for the sake of simplicity. It has been shown that using only the length of the strain path, the endochronic theory is capable of describing stress responses to complex strain paths. This version of endochronic theory is similar to but not quite the same as Ilyushin’s theory. One of the differences is in the deﬁnition of intrinsic time. The endochronic theory deﬁnes the intrinsic time by (7.70) using a material tensor Pijkm , whereas Ilyushin’s theory uses the arc length as the intrinsic time. Another difference, more signiﬁcantly, is that the endochronic theory is capable of accounting for volume change during deformation by use of the second equation of (7.72), while the theory of Ilyushin is formulated based on the deviatoric strain and no discussions have been given over to the volume change. It has been found that this version of endochronic theory does not correctly describe the unloading slope for metals and that it incorrectly predicts the same entropy production for further loading or unloading starting at a point already in the plastic state. Owing to the aforementioned deﬁciencies, an improved endochronic theory was developed by Valanis [2]. The new theory is free from the aforementioned deﬁciencies. In the new version, the intrinsic time is deﬁned by the plastic strain as p

p

dζ 2 = Pijkm dεij dεkm

(7.74)

The deviatoric part of the constitutive equation is σij

= 2G0

ζ 0

p

ρ(ζ − ζ )

dεij dζ

dζ

(7.75)

where G0 is a material constant and ρ(ζ ) is a kernel function. The volumetric change can be accounted for using the volumetric constitutive equation and the details of derivations are given in Chapter 8. It is shown in Chapter 8 that the ﬂow theory of plasticity may be derived from the new version of the endochronic theory. In addition, this theory is shown in Chapter 9 to apply to geotechnical materials which undergo plastic volume change during deformation.

7.6

Finite Plastic Deformation

Plastic deformations are large in cases such as metal forming, strain localization, ductile fracture, soil mechanics, and pavement analysis, etc. A plasticity

© 2005 by Chapman & Hall/CRC Press

358

Continuum Mechanics and Plasticity

theory of ﬁnite deformation must be used for these cases. The theories presented in previous sections of this chapter may be extended to the ﬁnite deformation range. The extension is not straightforward, however, and it has led to different opinions and heated debates. To extend an inﬁnitesimal theory into a ﬁnite theory, we encounter concepts such as the stress measure, the strain measure, the decomposition of strain into elastic and plastic parts, the objective rate (of stress, back stress, etc.), the observer independent yield function, and the rotation of material texture. The stress and strain measures and the decomposition of strain are discussed ﬁrst. The objective rate is then discussed in connection with hypoelasticity and discussion of its effects in plasticity is deferred until after a ﬁnite plasticity theory has been presented. Then the ﬁnite plastic simple shear deformation using different objective rates, and, ﬁnally, the yield function are discussed. 7.6.1

The Stress and Strain Measures

Either the Eulerian or the Lagrangian description may be used. The stress measures have already been discussed in Section 4.4.2.1 and strain measures in Sections 3.6, 3.9, and 3.10. In the Eulerian description, the stress and strains are referred to the current (deformed) conﬁguration. The Cauchy stress σ is usually used in this conﬁguration. This is the true stress, which is the force per unit deformed area. The Kirchhoff stress, which is deﬁned by Sij = Jσij where J is the Jacobian of the deformation equations, has also been used by some investigators. The Kirchhoff stress is also discussed in Chapter 11 in connection with the curvilinear coordinate system. Although we can use the Eulerian strain e or the left Cauchy–Green tensor B, it is more convenient to use the rate of deformation tensor D, which has the meaning of strain rate. The rate of deformation can be decomposed into the elastic and plastic parts and will be further discussed. In the Lagrangian description, the stress and strain refer to the undeformed (reference) conﬁguration. The nonsymmetric 1st P–K stress T(0) and the symmetric 2nd P–K stress have been used. Popular strain measures are the right Cauchy–Green tensor C and the Lagrangian strain (Green’s strain or Almansi strain) E. There is no uniﬁed approach available. The selection of the stress and strain measures greatly depends on the preference and convenience of the investigator and the problem at hand. 7.6.2

The Decomposition of Strain and Strain Rate

In the small deformation theory, it is customary to write p

εij = εije + εij

and

p

dεij = dεije + dεij

(7.76)

However, in ﬁnite deformation, the decomposition p

ERS = EeRS + ERS

© 2005 by Chapman & Hall/CRC Press

(7.77)

Advances in Plasticity

359

cannot be justiﬁed. This may be easily seen by considering the strain– displacement relation ERS

1 = 2

∂uR ∂uS ∂uk ∂uk + + ∂XS ∂XR ∂XR ∂XS

(7.78)

which cannot be separated into the sum of two parts because of the nonlinear terms in the displacement gradient. An additive decomposition was proposed by Green and Naghdi [56], who deﬁned Ee = E − Ep but explained that Ee was not an ordinary elastic strain tensor. It was deﬁned merely to represent the difference between the total strain E and the plastic strain Ep . The introduction of Ee was not necessary, because the use of E and Ep was sufﬁcient in their theory. On the other hand, the rate of deformation tensor can be separated into two parts because of the linear expression in the velocity gradient, that is, Dij = 12 (vi,j + vj,i )

(7.79)

p

It is possible to deﬁne two velocities vie and vi , such that Deij =

1 2

e e vi,j + vj,i

and

p

Dij =

1 2

p

p

vi,j + vj,i

(7.80)

Thus, p

Dij = Deij + Dij

(7.81)

We note that, in this connection, no attempt is made to separate the deformation gradient F into the elastic and plastic parts. In fact, F does not play a part in the formulation of (7.81). Another effort has been undertaken by researchers to derive the expressions of De and Dp starting from F. This effort involves some assumptions and physical justiﬁcations. Lee [57] introduced the concept of multiplicative decomposition of F. The deformation gradient has been previously discussed in Section 3.4. Let X express the initial conﬁguration of the body, x the elastic–plastic deformed state (the current conﬁguration), and p the state after de-stressing to zero stress. The deformation gradient F = ∂x/∂X with components FiR = ∂xi /∂XR expresses the total deformation. The deformation gradient Fp from the initial state X to the plastically deformed state p expresses the plastic deformation Fp =

© 2005 by Chapman & Hall/CRC Press

∂p ∂X

(7.82)

360

Continuum Mechanics and Plasticity

dx

F

X

x

dX

Fe

Fp dp

p X, x, p

FIGURE 7.23 Decomposition of F.

and Fe , from the plastically deformed conﬁguration p to x, expresses the elastic component of the deformation in the conﬁguration x, that is, Fe =

∂x ∂p

(7.83)

Thus, F = Fe · Fp

(7.84)

by the chain rule of differentiation. This decomposition of F into Fe and Fp is depicted by Figure 7.23. The intermediate conﬁguration p is obtained by an elastic de-stressing to zero stress from the current conﬁguration x and it represents a pure plastic deformation from X to p. If the plastic deformation is homogeneous, no residual stresses exist upon de-stressing and in this case Fe and Fp are continuous functions. However, if the plastic deformation is nonhomogeneous, residual stresses will result upon destressing. In order for all inﬁnitesimal material elements to reach a zero stress state, individual material elements will have to undergo a different amount of de-stressing. Therefore, in this case, Fe and Fp can be deﬁned as point-functions that relate the deformations in the inﬁnitesimal material elements. In addition, we mention that the intermediate state p is not uniquely deﬁned, because the elastic destressing can involve an arbitrary rigid-body rotation, which does not affect the stress. In order to have a unique p, we assume that the elastic de-stressing involves only pure deformation so that, by use of the polar decomposition of Section 3.5.2, the elastic part of the deformation gradient is Fe = Ve which is a symmetric tensor.

© 2005 by Chapman & Hall/CRC Press

(7.85)

Advances in Plasticity

361

Using (7.84) and (3.100), the Lagrangian strain is E = 12 (FT · F − 1) = 12 (FpT · FeT · Fe · Fp − 1) = 12 [FpT ·(FeT · Fe − 1)·Fp ] + 12 [FpT · Fp − 1] = FpT · Ee · Fp + Ep

(7.86)

where Ee = 12 (FeT · Fe − 1),

Ep = 12 (FpT · Fp − 1)

(7.87)

It is seen from (7.86) that the additive decomposition of Ee and Ep , as deﬁned here, does not hold, that is, E = Ee + Ep

(7.88)

The velocity gradient in the current conﬁguration x is L=

∂v ∂v ∂X = · = F˙ · F−1 ∂x ∂X ∂x

(7.89)

where F˙ is the material derivative of F. Substituting (7.84) into (7.89), we obtain −1 −1 −1 L = (Fe · Fp ) · (Fe · Fp )−1 = F˙ e · Fe + Fe · F˙ p · Fp · Fe

(7.90)

If we now choose the elastic de-stressing without rotation and the expression for Fe given by (7.85), and let −1 Lp = F˙ p · Fp = Dp + Wp

(7.91)

then ˙ e · Ve L=V

−1

+ V e · Dp · V e

−1

+ Ve · Wp · Ve

−1

(7.92)

From (7.92), the rate of deformation D and the spin tensor W take the form −1 −1 D = De + Ve · Dp · Ve S + Ve · Wp · Ve S −1 −1 W = We + Ve · Dp · Ve A + Ve · Wp · Ve A

(7.93)

where De , We (= 0, if Ve = VeT ), Dp , and Wp are the symmetric and antisym˙ e ·Ve−1 and Lp , respectively, and the subscripts S and A denote metric parts of V the symmetric and antisymmetric parts of a tensor. Looking at the expression for rate of deformation in (7.93), all three terms on the right-hand side of the equation are nonzero, in general. This indicates a very involved coupling of

© 2005 by Chapman & Hall/CRC Press

362

Continuum Mechanics and Plasticity

Ve , Dp , and Wp in combining to produce the total rate of deformation D. In this formulation, (7.92) cannot be reduced to the additive decomposition of D, expressed by (7.81), in the general case. However, elastic strain is small and negligible for most metals undergoing large plastic deformation, and we may use the approximation that Ve ≈ 1 to reduce (7.93) to D = De + Dp ,

W = We + Wp

(7.94)

On the other hand, Dafalias [58] introduced the concept of plastic spin based on Mandel’s concept of director vectors [59]. The plastic spin is a macroscopic representation of the rotation of material texture caused by plastic deformation. One way of observing the texture experimentally is to plot the pole ﬁgures. The rotation (or tilting) of texture has been observed experimentally by Montheillet et al. [60], Stout and O’Rourke [61], Toth et al. [62], and Wang et al. [63] in the torsion of thin-walled tubes or solid bars. Dafalias [64] further used the difference between the total spin W and the plastic spin Wp , termed constitutive spin ω to form the corotational rate. According to Dafalias, using Fe = Ve , (7.90) may be rewritten as ˙ e · Ve L=D+W =V = ω + Ve∇ · Ve

−1

−1

−1

+ Ve · F˙ p · Fp −1

+ Ve · Fp∇ · Fp

· Ve

· Ve

−1

−1

(7.95)

where the superscript ∇ denote the corotational rate, which has been discussed in Section 4.7.1. Since Ve transforms as a second-order tensor and Fp transforms as a vector upon the rotation of x (observer transformation), their corotational derivatives are ˙ e + Ve · ω − ω · Ve , Ve∇ = V

Fp∇ = F˙ p − ω · Fp

(7.96)

respectively. Restricting further to small elastic deformation for which Ve ≈ 1, the following are obtained from (7.95) −1

D = Ve∇ + (Fp∇ · Fp )S = De + Dp −1

W = ω + (Fp∇ · Fp )A = ω + Wp

(7.97)

with De = Ve∇ , rate of a symmetric elastic deformation; Dp and Wp the rates of plastic deformation and plastic spin, respectively. Thus, a portion of the total spin W is “absorbed” by the plastic spin and the rest accommodated by the constitutive spin ω. Dafalias [64] discussed the two deﬁnitions of “plastic spin” used in the literature and cautioned against deﬁning the plastic spin as the antisymmetric part of the velocity gradient at the plastically deforming intermediate conﬁguration. He suggested that the rotation of texture must be governed by a separate rule and not by the general kinematics of deformation. In the

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

363

continuum approach, constitutive equations must be provided not only for Dp but also for Wp , Mandel [59] and Kratochvil [65]. Dafalias writes Wp = λΩp (σ, s)

(7.98)

where λ is a parameter. An internal state variable s macroscopically describes the state of the microstructures. Using the representation theorem of Wang [66], Ωp can be represented by Ωp = η1 (s · σ − σ · s) + η2 (s · σ2 − σ2 · s) + η3 (σ · s · σ2 − σ2 · s · σ)

(7.99)

where η1 , η2 , and η3 are scalar valued functions of the invariants tr σ, tr σ2 , tr σ3 , tr(s · σ), and tr(s · σ2 ). Dafalias [64] and Loret [67] used the following simpliﬁed form to investigate the simple shear problem: Wp = η(α · σ − σ · α)

(7.100)

where η is a parameter and s is taken to be the back stress α. In addition, Dafalias [68] proposed the following form when he investigated plastic materials with kinematic hardening Wp = c(α · Dp − Dp · α)

(7.101)

where c is a parameter. EXAMPLE 7.1

Derive the corotational rate of vector g.

Solution Let g be subjected to an orthogonal transformation such that g¯ = QT · g

(a)

Dg¯ ˙ T · g + QT · g˙ =Q Dt

(b)

Then,

From the third equation of (4.92), we have ¯ = QT · W · Q + Q ˙ T · Q = QT · W · Q − Q T · Q ˙ W

(c)

˙ =W·Q−Q·W ¯ Q

(d)

or

© 2005 by Chapman & Hall/CRC Press

364

Continuum Mechanics and Plasticity

and ˙ T = QT · W T − W ¯ T · QT Q

(e)

Substituting (e) into (b), we obtain Dg¯ ¯ T · QT ) · g + QT · g˙ = (QT · WT − W Dt

(f)

¯ · g¯ = QT · (g˙ − W · g) g˙¯ − W

(g)

which leads to

It is to be noted that W is antisymmetric. The corotational rate of g can thus be deﬁned as ∇

g = g˙ − W · g

7.6.3

(h)

The Objective Rates

In Section 4.7 it was mentioned that only objective rates can be used to formulate a constitutive equation. There are many objective rates, however, and a reasonable objective rate should lead to results that can be veriﬁed by experiments. Different objective rates lead to different results and some are physically unacceptable results. For instance, it is known in hypoelasticity [69] that Jaumann rate gives rise to oscillatory shear and axial stresses with the increasing shear strain (see Section 4.10). In spite of this ﬁnding, some investigators continued to use the Jaumann rate in the ﬁnite deformation analysis. In the study of plasticity, Nagtegal and de Jong [70] analyzed the simple shear problem (shearing with constraint in axial direction) by use of the Jaumann rate for back stress using Prager’s linear kinematic-hardening rule. They showed an oscillatory shear stress response to monotonically increasing shear strain. This work triggered a series of investigations to look for objective stress rate appropriate for the description of metallic behavior in the ﬁnite strain range. Investigators have compared several objective stress rates with the purpose of eliminating the oscillatory stress–strain response. Yet, certain unreasonable behaviors, such as axial stress being zero or compressive with unacceptably large value, still exist in the available models. Furthermore, the majority of these models are for specimens subjected to loading only. When unloading or cyclic simple shearing are considered, the aforementioned unusual stress–strain behaviors can manifest itself in the unloading curve or the stress–strain loops. Discussions have been centered around two possibilities of eliminating the oscillatory behavior. One is to ﬁnd an objective rate that does not give rise to oscillatory stress responses even using a linear

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

365

constitutive equation. The other is to add a nonlinear term to the constitutive equation and, in this case, Jaumann rate does not lead to oscillatory stresses. In this subsection, the objective rate is discussed in connection with hypoelasticity. The effect of objective rate in plasticity is deferred to a later section. In the case of simple shear deformation, the hypoelastic constitutive equation is from (4.240) σij∗ = 2µDij

and

Dkk = 0

(7.102)

where σ∗ an objective rate and µ is the shear modulus. The simple shear deformation is governed by the following equations x1 = X1 + 2ωtX2 , u1 = 2ωtX2 ,

0 [L] = 0 0

0 0 , 0

2ω 0 0

x2 = X2 ,

u2 = u3 = 0,

0 [D] = sω 0

ω 0 0

x3 = X3

(7.103)

ω = const

(7.104)

0 0 , 0

0 [W ] = −ω 0

ω 0 0

0 0 0 (7.105)

The case of σ∗ equaling to the Jaumann rate σ∇ = (Dσ/Dt) − W · σ + σ · W has been discussed in Section 4.10. Following the procedures of Section 4.10, This section discusses the solutions of (7.102) and (7.105) using the Cotter–Rivlin stress rate [71], Oldroyd’s convected stress rate [72], the Green–McInnis rate [69], and the mixed objective stress rates. In the case of the Cotter–Rivlin stress rate, the stress rate is σ∗ =

Dσ + LT · σ + σ · L Dt

(7.106)

and the solution is σ11 = 0,

σ22 = −4µγ 2 ,

σ12 = 2µγ

(7.107)

where γ = 2ωt. Note that σ12 increases linearly and σ22 nonlinearly with γ . Even though the shear stress–strain curve does not oscillate, which satisﬁes the requirement, the magnitude of the axial stress is greater than that of the shear stress. According to the experimental ﬁndings of Montheillet et al. [60], White and Anand (reported in [73]), and Wu et al. [74], the magnitude of axial stress is about 10% of shear stress. The predicted high σ22 of this model makes the model unacceptable. In the case of Oldroyd’s rate, the stress rate is σ∗ =

© 2005 by Chapman & Hall/CRC Press

Dσ − L · σ − σ · LT Dt

(7.108)

366

Continuum Mechanics and Plasticity

On the other hand, Truesdell’s rate [75] is σ∗ =

Dσ + σ tr D − L · σ − σ · LT Dt

(7.109)

Since tr D = 0, (7.109) reduces to (7.108). The solution of this case is σ11 = 4µγ 2 ,

σ22 = 0,

σ12 = 2µγ

(7.110)

This model predicts a zero σ22 and a high magnitude of σ11 which are unacceptable for real materials. Using the Green–McInnis rate σ∗ =

Dσ − W∗ · σ + σ · W∗ Dt

˙ · RT where W∗ = R

(7.111)

in which tensor R is the orthogonal rotation tensor of the polar decomposition of the deformation gradient F, Dienes [69] obtained the following solution σ11 = −σ22 = 4µ[cos 2β ln(cos β) + β sin(2β) − sin2 β] σ12 = 2µ cos 2β[2β − 2 tan 2β ln(cos β) − tan β]

(7.112)

where tan β = ωt = 12 γ

(7.113)

The shear stress–strain curve of this model does not oscillate but the magnitude of axial stress is in the order of shear stress and does not agree with the experimental ﬁnding of approximately one-tenth of the magnitude of the shear stress. All the aforementioned solutions of hypoelasticity are plotted in Figure 7.24. EXAMPLE 7.2

Use the Green–McInnis rate to ﬁnd the stresses for simple

shearing. Solution The motion for simple shearing is from (3.20) x1 = X1 + 2X2 tan β,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(a)

Advances in Plasticity

367 Jaumann 22 = J22 Truesdell 22 = 0 Cotte–Rivlin 22 = C22 Dienes 22 = D22

Jaumann 12 = J12, Truesdell 12 = T12, Cotter–Rivlin 12 = C12, Dienes 12 = D12,

Stress MPa 60

C12, T12 D12

40 20

J12

–2

–4

4

2 D22

J22 C22

–60

FIGURE 7.24 Simple shear of hypoelastic material.

From (a), we ﬁnd

1 [F] = 0 0

2 tan β 1 0

0 0 , 1

1 2 T [U ] = [F] [F] = 2 tan β 0

0

[D] = sec2 β β˙ 0 2 tan β 0 4 tan2 β + 1 0 0 1

sec2 β β˙ 0 0

0 0 , 0

(b)

The eigenvalues and eigenvectors of [U 2 ] are λ2 = 1 + 2 tan2 β + 2 tan β sec β,

λ1 = 1,

λ3 = 1 + 2 tan2 β − 2 tan β sec β n1T = 0 n3T

0

1 ,

[(2 tan β − sec β) − 2 1] , n2T = (2 tan β − sec β)2 + 5

[(2 tan β + sec β) − 2 1] = (2 tan β + sec β)2 + 5

(c)

Therefore, [U] is

1

[U] = [n1

© 2005 by Chapman & Hall/CRC Press

n2

0

n3 ] 0

λ2

0

0

1/2

0

n1T

0 n2T 1/2 n3T λ3

(d)

368

Continuum Mechanics and Plasticity

We ﬁnd

[R] = [F][U]−1

cos β = − sin β 0

sin β cos β 0

0 0 , 1

sin β β˙ ˙ [R] = − cos β β˙ 0

cos β β˙ − sin β β˙ 0

0 0 0 (e)

and

0 T ˙ [w∗ ] = [R][R] = β˙ 0

β˙ 0 0

0 0 0

(f)

Using the Green–McInnis rate (7.111), the nonzero components of (7.102) are dσ11 ˙ 12 = 0 − 2βσ dt dσ12 ˙ 11 − σ22 ) = 2µ sec2 β β˙ + β(σ dt dσ22 ˙ 12 = 0 + 2βσ dt

(g) (h) (i)

Equations (g) to (i) are combined to yield d2 σ11 4µ + 4σ11 = dβ 2 cos2 β

with σ22 = −σ11

(j)

The general solution for (j) is σ11 = 4µ(cos 2β ln cos β + β sin 2β − sin2 β) + c1 cos 2β + c2 sin 2β

(k)

where c1 and c2 are constants and they vanish when all initial (at β = 0) stress components are zero. Substituting (k) into (g), gives (7.112).

7.6.4

A Theory of Finite Elastic–Plastic Deformation

The rate of deformation D is used in this section. According to the concept of work conjugate discussed in Section 4.4.3, the Cauchy stress σ is the work conjugate of D. An objective stress rate should be used and we use the Jaumann rate in this discussion. Other objective stress rates will be discussed in the next section. The Jaumann stress rate is σij∇ = σ˙ ij − Wip σpj + σip Wpj

© 2005 by Chapman & Hall/CRC Press

(7.114)

Advances in Plasticity

369

where σ˙ ij = Dσij /Dt. Denoting the deviatoric part of Dij by dij , we have p dij = dije + dij . The Mises yield criterion is f = ξijD ξijD −

2Y 2 =0 3

(7.115)

where ξijD = σij − αijD ; the superscript D denotes the deviatoric part of the quantity and Y is the current yield stress in tension. The plastic region is p characterized by f = 0 and dij dσij > 0, while the elastic region is characterized p

by either f < 0 or f = 0 and dij dσij ≤ 0. The tensor αij is the back stress. The elastic behavior is governed by σij ∇ = 2µdije

(7.116)

where µ is the shear modulus. The ﬂow rule is p dij = λ˙

∂f ∂σij

(7.117)

where λ˙ is a scalar factor of proportionality. Using (7.115), (7.117) reduces to p ˙ ijD dij = λξ

(7.118)

For simplicity, the linear isotropic-hardening rule is used and is written as Y˙ = βhd¯ p

(7.119)

where d¯ p is the equivalent plastic strain rate deﬁned by d¯ p =

p p 1/2 3 dij dij

2

(7.120)

and h is the slope of isotropic-hardening curve. The parameter β was previously discussed in (6.85) and β = 1 for isotropic hardening. Prager’s linear kinematic-hardening rule is used, that is, p

αijD∇ = 23 (1 − β)hdij

(7.121)

where β = 0 or kinematic hardening. The parameter β lies within 0 ≤ β ≤ 1. When β has a value between 0 and 1, then we have a combined isotropic– kinematic hardening.

© 2005 by Chapman & Hall/CRC Press

370

Continuum Mechanics and Plasticity

The factor λ˙ is determined from the consistency condition. Differentiating (7.115), gives 4Y ˙ f˙ = 2ξijD ξijD∇ − Y=0 3

(7.122)

The expressions in (7.122) can be shown as p ξijD ξijD∇ = ξijD σij ∇ − αijD∇ = ξijD 2µdije − 23 (1 − β)hdij = 2µdij ξijD − 2µ + 23 (1 − β)h λ˙ 23 Y 2 2 2 D D 1/2 2 ˙ 2 2 ¯p ˙ = 49 βhY 2 λ˙ 3 Y Y = 3 Yβhd = 3 Yβh 3 λ ξij ξij

(7.123)

By substituting the two expressions of (7.123) into (7.122), we obtain 2µdij ξijD = 23 λ˙ Y 2 2µ + 23 (1 − β)h + 23 βh

(7.124)

which may be solved for λ˙ to obtain λ˙ =

dij ξijD 3 2 Y 2 (1 + (h/3µ))

(7.125)

˙ the rate of deformation may now be Having found the expression for λ, written as p

dij = dije + dij =

σij ∇ 2µ

+

D D 3 dkm ξkm ξij 2 Y 2 (1 + h/3µ)

(7.126)

This equation may be inverted to obtain σij ∇

= 2µ δik δjm −

D ξD ξkm ij

(2/3)Y 2 (1 + h/3µ)

dkm

(7.127)

that is, the stress rate is expressed in terms of the rate of deformation dij . This equation is often written as σij ∇ = Lijkm dkm

(7.128)

to facilitate computation. We note that the volumetric behavior is assumed to be elastic which is described by 1 ˙ kk 3σ

where K is the bulk modulus.

© 2005 by Chapman & Hall/CRC Press

= KDkk

(7.129)

Advances in Plasticity

371

Using the theory of this section to derive the stress–strain relation for uniaxial stress.

EXAMPLE 7.3

Solution In the case of uniaxial stress 2 0 0 3σ σ

[σ ] = 0 0 −3 , σ 0 0 − 3 2α 0 0 3 α [α D ] = 0 − 0 3 α 0 0 3

ε˙ p

[Dp ] = [dp ] = 0 0

0 1 p − ε˙ 2 0

0

0 1 p − ε˙ 2

(a)

Using (a), the yield function (7.115) is reduced to σ =Y+α

(b)

and, using (7.125), the equivalent plastic strain rate is d¯ p = { 23 [(˙ε p )2 + 2(− 12 ε˙ p )2 ]}1/2 = ε˙ p

(c)

The linear isotropic-hardening rule is then given by Y˙ = βh˙εp

(d)

and the linear kinematic-hardening rule is from (7.121) and (7.130) reduces to α˙ = (1 − β)h˙ε p

(e)

˙ and αD∇ = α˙ D . The expression for (d) is the We note that due to W=0, σ∇ = σ, same as (6.147) and the expression for (e) is the same as (6.149). The roles of isotropic and kinematic hardening are similar to those shown in Figure 6.21(b). Using (d) and (e), the stress–plastic strain curve is given by σ˙ = Y˙ + α˙ = βh˙εp + (1 − β)h˙ε p = h˙εp

(f)

The slope of the stress–plastic strain curve may be identiﬁed as h=

© 2005 by Chapman & Hall/CRC Press

σ˙ dσ = p ε˙ p dε

(g)

372

Continuum Mechanics and Plasticity

where the slope is a function of ε p . The total strain is σ˙ σ˙ ε˙ = ε˙ + ε˙ = + = E h e

p

1 1 + σ˙ E h

(h)

where E is the elastic modulus. In the stress–strain curve, the slope is 1 dσ = = Et dε (1/E) + (1/h)

(i)

where Et is the tangent modulus. Therefore, Et =

hE h+E

(j)

This equation relates Et to E and h. Using (i), the axial stress–strain curve may be plotted. It is noted that the ﬂow rule is not explicitly used in this one-dimensional case. A rectangular metal block with edges parallel to the x, y, z-axes is compressed in the x-direction between overlapping rigid plates. Expansion is allowed only in the y-direction, and is prevented in the z-direction by rigid dies. All contact surfaces are perfectly lubricated so that the deformation is plane and uniform. The compressive strain in the x-direction is controlled and it increases monotonically from zero. Determine the stresses. Use the theory of this section and assume that the material hardens only by isotropic hardening.

EXAMPLE 7.4

Solution Assume that in the elastic region, the behavior is hypoelastic so that p σ˙ ij = λδij Dkk + 2µ Dij − Dij

with Dkk = Dekk

(a)

We note that since W = 0 for this problem, σij∇ = σ˙ ij . The ﬂow rule is ˙ ij

Dij = φσ p

p

(b)

p

where Dij = dij due to plastic incompressibility. Parameter φ is used here so that a distinction can be made between this parameter and the Lamé constant λ used in (a). The equivalent plastic strain rate is ¯p = D

© 2005 by Chapman & Hall/CRC Press

p p 1/2 3 Dij Dij

2

(c)

Advances in Plasticity

373

and the yield function is 2Y 2 =0 3

f = σij σij −

(d)

with the consistency condition 4Y ˙ f˙ = 2σij σ˙ ij − Y=0 3

(e)

The isotropic hardening is ¯ p, Y˙ = hD

β=1

(f)

Dij σij

3 2 Y 2 (1 + h/3µ)

(g)

Using (7.125), we obtain φ˙ =

Substituting (g) and (b) into (a), we ﬁnd

σij

σ˙ ij = λδij Dkk + 2µDij − BDkm σkm

(h)

where B=

3µ Y 2 (1 + h/3µ)

(i)

The boundary conditions are σx = 0,

σy = 0,

σz = 0,

Dx = 0 (known),

Dy = 0, Dz = 0 (j)

Apply the conditions σ˙ y = 0 and Dz = 0 in (h) gives Dy = −

C1 Dx C2

(k1)

where

© 2005 by Chapman & Hall/CRC Press

C1 = 3λ + B(σx + σz )(2σx − σz )

(k2)

C2 = 3λ + 6µ − B(σx + σz )2

(k3)

374

Continuum Mechanics and Plasticity

The other two components of (h) are σ˙ x = λ(Dx + Dy ) + 2µDx − A(2σx − σz )

(l1)

σ˙ z = λ(Dx + Dy ) − A(2σz − σx )

(l2)

where A=

−1 σx + σ z

[λ(Dx + Dy ) + 2µDy ]

(l3)

and (k1) was used in the derivation of (l3). Equations (l1) to (l3) can be further reduced to σ˙ x = C3 Dx + C4 Dy

(m1)

σ˙ z = C5 Dx + C6 Dy

(m2)

where

3σx C3 = 2µ + λ σx + σ z 3σz C5 = λ , σx + σ z

σx − 2σz , C4 = C3 + 2µ σx + σ z σx − 2σz C6 = C5 − 2µ σx + σ z

(m3)

Finally, we substitute (k1) into (m1) and (m2) to obtain

C 1 C4 σ˙ x = C3 − C2

Dx

and

C 1 C6 σ˙ z = C5 − C2

Dx

(n)

It is to be noted that Ci are functions of σx , σz and material constants. If we know Dx , then σx and σz may be calculated by the integration of (n), and Dy may be found from (k1). Additional exercises may be performed by plotting the σx versus Dx dt and σz versus Dx dt curves. In addition, Dy may be plotted as a function of Dx and the effect of h on the results discussed. An experimental study of the biaxial compression problem was conducted by Khan and Wang [76].

7.6.5

A Study of Simple Shear Using Rigid-Plastic Equations with Linear Kinematic Hardening

The subject of study in this section is the problem of simple shear using rigid-plastic equations with linear kinematic hardening, that is, β = 0. Three objective rates are considered. They are the Jaumann rate, the Dafalias rate, and Lee’s rate [77].

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

375

7.6.5.1 The Jaumann rate The Mises yield criterion is 3

2 (σ

− αD ) · (σ − αD ) = Y 2

(7.130)

The kinematic-hardening rule is from (7.121) αijD∇ = 23 hDij

(7.131)

p

where dij = dij = Dij and Dkk = 0. The Jaumann rate is given by (7.114) and the ﬂow rule is from (7.118) Dij = λ˙ σij − αijD

(7.132)

Using the ﬁnite simple shear straining described by (7.105), we obtain from (7.132)

D σ11 = α11 ,

D σ22 = α22 ,

D σ12 = α12 +

ω Y D +√ = α12 λ˙ 3

(7.133)

The last expression was obtained using (7.132) and (7.130). The expression of (7.131) is in the form of (7.102), whose solution in the case of Jaumann rate is given by (4.248). Therefore, the solution for (7.131) is D α12 =

h sin γ , 3

D D = −α22 = α11

h (1 − cos γ ) 3

(7.134)

D + α D = 0 and, therefore, from the ﬁrst two From (7.134) we infer that α11 22

= −σ or (2σ − σ )/3 = −(2σ − σ )/3. equations of (7.133) we obtain σ22 22 11 11 22 11 Thus, σ11 + σ22 = 0 or σkk = 0, since σ33 = 0. Using this result, we conclude

and σ = σ . Equations (7.133) and (7.134) combine to yield that σ11 = σ11 22 22

Y h σ12 = √ + sin γ , 3 3

σ11 = −σ22 =

h (1 − cos γ ), 3

other σij = 0 (7.135)

This is the solution for the simple shear problem by use of the Jaumann rate for the back stress. It is seen that all nonzero stress components are oscillatory. Finally, it is easy to show that by eliminating γ from the equations of (7.134), we ﬁnd

D α12

2

+

h D − α11 3

2

=

2 h 3

(7.136)

that is, the back stress is making a circular motion when the Jaumann rate is used.

© 2005 by Chapman & Hall/CRC Press

376

Continuum Mechanics and Plasticity

7.6.5.2 The Dafalias rate The yield function is given by (7.130) and the ﬂow rule is given by (7.132). Upon the substitution of (7.105) into (7.132), we obtain (7.133). The kinematichardening rule is ∗

αijD = 23 hDij

(7.137)

in which ∗

αijD =

DαijD Dt

− ωij αjiD + αijD ωji

(7.138)

is the Dafalias rate; ωij is the constitutive spin deﬁned by (7.97) and is written as p ωij = Wij − Wij = Wij − η αijD Dji − Dij αjiD

(7.139)

where η is a parameter which describes the strength of plastic spin. By use of (7.105), it is easily shown that

0 [ω] = ξ −ω 0

0 0 0

ω 0 0

D D with ξ = 1 − η α11 − α22

(7.140)

Thus, (7.137) is reduced to

D α11

D α D Dt 12 0

D α12 D α22

0

0

D 2α12

D D 0 − ξ ω α22 − α11 0 0

D − αD α22 11 D −2α12

0

0 0 2 ω h = 0 3 0 0

ω 0 0

0 0 0

(7.141) The nonzero components of the equation are D Dα11 D D D 1 − ηα11 ω + ηα22 = 2α12 Dt D Dα22 D D D 1 − ηα11 ω + ηα22 = −2α12 Dt D D Dα12 2 D D D 1 − ηα11 ω − α11 + ηα22 = hω + α22 3 Dt

© 2005 by Chapman & Hall/CRC Press

(7.142)

Advances in Plasticity

377

D = α D = 0 initially, α D = −α D for all t. Using this result, (7.142) is Since α11 22 11 22 simpliﬁed to yield D D dα11 D α12 , = 1 − 2ηα11 dγ

D D dα12 h D α11 = − 1 − 2ηα11 dγ 3

(7.143)

D /Y and where γ = 2ωt. We now introduce dimensionless variables αˆ 11 = α11 D αˆ 12 = α12 /Y, and a parameter hˆ = h/(3Y), so that (7.143) may be written as

dαˆ 11 ˆ αˆ 11 )αˆ 12 , = (1 − hρ dγ

dαˆ 12 ˆ αˆ 11 )αˆ 11 = hˆ − (1 − hρ dγ

(7.144)

where ˆ = 2ηY hρ

(7.145)

The equations in (7.143) are solved numerically by Dafalias [58]. The boundary condition is αijD = 0 at initial yielding. Similar to (7.133), we may establish that D σ11 = α11 ,

D D σ22 = α22 = −α11 ,

Y D σ12 = α12 +√ 3

(7.146)

In Figure 7.25(a), we plot the shear stress–strain curves with values of hˆ = 1.0, 1.5, 1.6, 1.7, 1.75, and 2.0, while keeping ρ = 0.08. The corresponding axial stress versus shear strain curves are plotted in Figure 7.25(b), and the corresponding back stress paths as the shear strain γ increases are plotted in Figure 7.25(c). It clearly shows that the solution is very sensitive to the relative value between hˆ and ρ. A large ρ indicates a strong plastic spin and the corresponding constitutive spin is small. When hˆ is relatively small such as 1.0, the constitutive spin is signiﬁcant and it causes the back stress to spin as indicated in Figure 7.25(c). As a result, both the axial and shear stresses are ˆ but they are very oscillatory. The stresses are not oscillatory for larger h, sensitive to this parameter as seen from Figure 7.25(b) and (c). We would also like to mention that generally the magnitude of axial stress of this model is larger than the shear stress, which is not reasonable. 7.6.5.3

The rate of Lee

Lee et al. [77] proposed a spin W∗ to replace the spin tensor W in the Jaumann rate, achieving nonoscillatory stresses in simple shearing. The tensor W∗ is determined by the angular velocity of the material line element which is instantaneously coincident with the eigenvector associated with the maximum eigenvalue of back stress α. The spin W∗ is expressed by Wij∗ = Wij + Dik nk nj − ni nk Dkj

© 2005 by Chapman & Hall/CRC Press

(7.147)

378

Continuum Mechanics and Plasticity (a)

4

5

2.0

1.7

7

1.

12 /Y

3 2

1.0

1.6

1 2

6

4

8

10

–1 15 –2 (b)

6

1.7

1.75

1.6

5 0

2.

11/Y

4

1.

5

3 2

1.

0

1 2

–1

4

6

8

10

–2 (c) 2.0

12.5

12 /Y

10 1.75

7.5 5

1.7

2.5 1

1.0 3

5

1.6 /Y 7 11

1.5 FIGURE 7.25 Simple shear using Dafalias’s rate: (a) shear stress–strain curves, (b) axial stress, (c) back stress.

where n is that eigenvector of α. Lee et al. [77] pointed out that kinematic hardening is an anisotropic phenomenon for which speciﬁc directions embedded in the material and the rotation of these particular directions play a signiﬁcant role. It is noted, however, that the rotation of the eigenvector used to deﬁne W∗ is a part of the kinematics of deformation and is not directly related to the rotation of the material texture. Dafalias rate is different

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

379

in that it contains a parameter that is related to the spin of the material texture. Following [77], we now use W∗ in connection with the corotational rate to investigate the simple shear deformation. The rate of Lee et al. may be written as ∗

αD =

DαD − W ∗ · αD + α D · W ∗ Dt

(7.148)

Since a corotational rate is objective, Lee’s rate is objective. For the simple shear deformation deﬁned by (7.105), the line element associated with W∗ is on the (x1 , x2 ) plane. Thus, [n]T = [n1 n2 0]. Substituting this expression of [n] into (7.147), we ﬁnd

1 0 0 0 0 0

0 [W ∗ ] = 2n22 ω −1 0

with n21 + n22 = 1

(7.149)

Using (7.149) and (7.148), the nonzero components of the linear kinematichardening rule (7.137) are D D α˙ 11 − 4n22 ωα12 =0 D D α˙ 22 + 4n22 ωα12 =0

(7.150)

D 2h D D α˙ 12 − 2n22 ω α22 − α11 = ω 3 Equations in (7.150) are further reduced to D = α˙ 12

2h D ω − 4n22 ωα11 , 3

D D α˙ 11 − 4n22 ωα12 = 0,

D D and α22 = −α11

(7.151)

We now determine the eigenvector n. We have

D −λ α11

D α12 0

0 n1 0 n2 = 0 0 0 0−λ

D α12

0

D −λ α22

0

(7.152)

From (7.152), we obtain n1 = 1 − n22 ,

n2 =

1 R2 + 1

,

R=

D + −α22

D α22

2

D 2 + α12

D α12

(7.153)

© 2005 by Chapman & Hall/CRC Press

380

Continuum Mechanics and Plasticity 2.0

(a)

1.5

12/ Y

6

1.0

4 2

2

4

8

6

(b) 12

2.0

10

1.5

8 11/Y

10

6

1.0

4 2

2 (c)

4

8

6

10

7

2.0

6 12/Y

5

1.5

4

1.0

3 2 1

2

4

6

11/Y

8

10

12

FIGURE 7.26 Simple shear using Lee’s rate: (a) shear stress–strain curves, (b) axial stress, (c) back stress.

The positive n2 is chosen which corresponds to the maximum eigenvalue. D and α D . Knowing In this way, n2 is expressed in terms of components α22 12 D αij , we determine [n], which may then be substituted into (7.151). Finally, we mention that (7.146) still applies in this case. Numerical results for simple shear using Lee’s rate are plotted in Figure 7.26(a) to (c). The curves are plotted for hˆ = 1.0, 1.5, and 2.0. We see that all curves are not oscillatory, but the predicted axial stress is too large.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity EXAMPLE 7.5

381

Show that W∗ of Lee’s rate represents the spin of a material

line element. Solution Let the line element be dxi and be denoted by dxi = ni ds

(a)

where ni is the unit vector along the line element and ds is the length of the line element. The relative velocity between the ends of the line element is dvi =

∂vi dxj = Lij nj ds ∂xj

(b)

The component of dv normal to n determines the spin W* of that line element to within an arbitrary spin. The component of dv normal to n is denoted by dv∗ = dv − (dv · n)n

(c)

Then, (c) in the subscript notation is dvi∗ = dvi − dvk nk ni = Lij nj ds − Lkj nj dsnk ni = (Dij + Wij )nj ds − (Dkj + Wkj )nj nk ni ds = Dij nj ds + Wij nj ds − Dkj nj nk ni ds

(d)

dv∗ = w∗ × n ds

(e)

But,

where w∗ is the dual vector of W∗ . In the index notation, (e) is dvi∗ = eijk wj∗ nk ds = ekij wj∗ nk ds = −Wki∗ nk ds = Wik∗ nk ds

(f)

Equating (d) and (f), we obtain Wik∗ nk = Dij nj (nk nk ) + Wij nj − Dkj nj nk ni

(g)

Wij∗ = Wij + Dik nk nj − ni nk Dkj

(h)

which reduces to

© 2005 by Chapman & Hall/CRC Press

382

Continuum Mechanics and Plasticity

EXAMPLE 7.6

Let the simple shear motion be

0 [D] = ω 0

ω 0 0

0 0 , 0

0 [W ] = −ω 0

ω 0 0

0 0 0

(a)

Find the expression of [W*]. Solution Let [n] = (cos θ , sin θ , 0), then from (7.147)

0 [W ∗ ] = −2ω sin2 θ 0

0 0 0

2ω sin2 θ 0 0

(b)

Since wk∗ = − 12 eijk Wij∗

(c)

We ﬁnd [w∗ ]T = 0

0

−2ω sin2 θ

(d)

Thus, the angular velocity w3∗ = θ˙ of the line element varies with the direction of the line element deﬁned by angle θ . The line along the x1 -axis does not rotate and the spin is maximum along the x2 -axis. 7.6.5.4

Remarks about objective rates of plasticity

The spin W is overemphasized by the Jaumann rate. In simple shear, W is the angular velocity θ˙ of the line element, along the principal direction of D, making a θ = π/4 angle with the x1 -axis. Referring to Figure 7.27, a square material element initially at OA0 B0 C assumes the shape OABC during simple shearing. As the shear strain becomes large, all lines emanating from O and lying within the angle ∠AOC have small angles θ, which are less than π/4. According to Lee et al. [77], these lines do not have the same θ˙ and do not rotate much. The line along OC does not spin at all and the line along OA does not spin as much as W. This effect may be seen from Example 7.5 by using a small θ in equation (d). It is noted that both Dij and Wij refer to a square element, with sides parallel to the x1 and x2 axes, deﬁned at the current conﬁguration. Therefore, W represents the spin of this new element which does not contain the same material mass as the original element. The Jaumann rate overemphasizes W because it does not represent the spin of the original material element.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

383

x2

1

A0

0

B0

C

A

B

x1

FIGURE 7.27 Rotation of line element during simple shearing.

From the discussions of previous subsections, we see that some objective rates lead to oscillatory stress components in simple shearing when the shear strain is monotonically increasing. This effect is of course in violation of experimental observations. Of the several objective rates discussed none can lead to acceptable stress responses using a linear kinematic-hardening equation. Several rates lead to an axial stress which is about the same or larger in magnitude than the shear stress, while experimental results show that the axial stress is about one-tenth of the magnitude of the shear stress. A conclusion may be drawn that these rates will have to be applied to a nonlinear kinematic-hardening equation. The concept of constitutive spin proposed by Dafalias [64] is promising. It introduces a constitutive equation for the plastic spin which is a macroscopic description of the spin of material texture. From the experimental investigation of material textures [60–63], it is known that the spin (or tilting) of the material texture is not directly expressed by the general kinematics of deformation. In the case of torsion, for instance, a monotonic increasing shear deformation can cause the texture to rotate in a direction of decreasing shear strain and then reverse its direction as the shear strain becomes larger. This is the evidence that plastic spin should not be deﬁned by the general kinematics of deformation. The plastic deformation induced anisotropy is described to a large extent by the kinematic hardening. Since plastic deformation changes the material texture, it is reasonable to use the back stress to describe the texture rotation. As previously mentioned, the plastic spin is independent of the kinematics of deformation, while the stress rate and the strain rate are dependent of the same. Therefore, different objective rates should be used for back stress, stress, and strain. In Wu [78,79], we use Dafalias rate for the back stress, and the convected rate for the stress and strain. This approach will be further discussed in Chapter 11 in connection with a curvilinear coordinate system.

© 2005 by Chapman & Hall/CRC Press

384 7.6.6

Continuum Mechanics and Plasticity The Yield Criterion for Finite Plasticity

Most works of ﬁnite plasticity have focused on the decomposition of deformation into elastic and plastic parts and the objective stress rates or back stress rates. Little attention has been given to the yield criterion applicable in the ﬁnite deformation range. Most theoretical works have assumed that the Mises yield criterion can be used. Some apply the Mises criterion expressed in terms of the Cauchy stress and some the 2nd P–K stress. The main concern is that yield criterion should be observer independent. For an isotropic material, this statement is equivalent to the requirement that the yield criterion be independent of rigid-body rotation of the material element. However, this is only an approximation because the material does not remain isotropic during plastic deformation. A yield criterion is observer independent, if it is deﬁned by stress invariants. It is noted, however, that a square material element used to deﬁne the Cauchy stress does not remain square during plastic deformation. If referring to the orientation of another observer, a square element is chosen to describe the state of stress, the aforementioned two square elements do not contain the same material mass. The two elements can be compared only when material isotropy is assumed and the concept of stress invariants is based on this assumption. In Chapter 11, an observer independent yield criterion will be deﬁned in terms of the contravariant true stress, which remains unchanged either during an observer transformation or when the material element undergoes a superimposed rigid-body rotation. In the remainder of this section, we investigate the effect of stress measure on the shape, size, and translation of the yield surface when the specimen has been prestrained into the ﬁnite deformation range. Speciﬁcally, we compare the yield surfaces in the combined axial–torsion problem when the yield function is deﬁned by the Cauchy stress, the 1st P–K stress, and the 2nd P–K stress, following the study of Wu et al. [24]. Usually, the stresses in the experimental data are the physical components in the cylindrical-coordinates system, so that all stress components have the same unit. The physical components will be discussed in Chapter 11 in connection with the curvilinear coordinates. The physical components in the present case are components of a tensor referred to unit vectors er , eθ , ez in the radial, tangential, and axial direction, respectively. Determine the physical components of the deformation gradient F in the cylindrical coordinate system.

EXAMPLE 7.7

Solution Let (r, θ , z) be the cylindrical coordinates of a point having Cartesian coordinates (x, y, z). The following equations hold x = r cos θ ,

© 2005 by Chapman & Hall/CRC Press

y = r sin θ,

z=z

(a)

Advances in Plasticity

385

An inversion of (a) yields r 2 = x2 + y 2 ,

θ = tan−1

y x

z=z

,

(b)

The unit base vectors of the cylindrical system are (er , eθ , ez ), and the unit vectors of the Cartesian system are (ex , ey , ez ). These unit vectors are related by er = cos θex + sin θey ,

eθ = − sin θex + cos θey

(c)

Taking the partial derivatives of (b) and using (a), we obtain ∂r x = = cos θ, ∂x r

∂r y = = sin θ, ∂y r

∂θ −y −y − sin θ = 2 = 2 = , 2 ∂x r x +y r

∂θ cos θ = ∂y r

(d)

Differentiation of (c) gives ∂eθ ∂ez ∂ez ∂er ∂eθ ∂ez ∂er = = = = = = =0 ∂r ∂r ∂r ∂θ ∂z ∂z ∂z ∂eθ ∂er = eθ , = −er ∂θ ∂θ

(e)

Consider now the undeformed position vector P and the current position vector p of a point expressed in the cylindrical system as P = ReR + ZeZ ,

p = rer + zez

(f)

where (R, Z) and (r, z) are components of the undeformed and deformed position vectors, respectively; (eR , eZ ) and (er , ez ) are the unit vectors of the two systems. Using (e), the differential forms for (f) are dP = dReR + R de + dZeZ ,

dp = drer + rdθeθ + dzez

(g)

We now proceed to ﬁnd a relation between the components of dp and those of dP. To this end, we note that r, θ, z are functions of R, , Z. Thus, by chain rule of differentiation, we obtain ∂r ∂r ∂r dR + R d + dZ ∂R R∂ ∂Z r∂θ r∂θ r∂θ dR + Rd + dZ r dθ = ∂R R∂ ∂Z ∂z ∂z ∂z dz = dR + Rd + dZ ∂R R∂ ∂Z dr =

© 2005 by Chapman & Hall/CRC Press

(h)

386

Continuum Mechanics and Plasticity

Using (h), the components of (g) may be written in matrices as

∂r ∂R dr r∂θ [dp] = r dθ = ∂R dz ∂z ∂R

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂Z dR r∂θ R d = [F][dP] ∂Z dZ ∂z ∂Z

(i)

where the components of the deformation gradient are

∂r ∂R r∂θ [F] = ∂R ∂z ∂R

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂Z r∂θ ∂Z ∂z

(j)

∂Z

7.6.6.1 Relations among stress measures for thin-walled tubes The text of this section was originally presented in [24]. Considering the axial– torsion of a thin-walled tube, two sets of cylindrical coordinates (X 1 , X 2 , X 3 ) = (R, , Z) and (x1 , x2 , x3 ) = (r, θ, z) are used to describe the undeformed and deformed status, respectively. The two sets of coordinates are related by r = λm Rm − λ2 (Rm − R) = (λm − λ2 )Rm + λ2 R θ = + ϕλ3 Z

(7.154)

z = λ3 Z in the range of R1 ≥ R ≥ R0 , where R1 and R0 are the undeformed outer and inner radii, respectively; and r1 ≥ r ≥ r0 , where r1 and r0 are the deformed outer and inner radius, respectively; λm = rm /Rm describes the stretch ratio of the mean radii which are denoted by Rm and rm in the undeformed and deformed status, respectively; λ2 = h/H describes the stretch ratio of the wallthicknesses, which are denoted by H and h in the undeformed and deformed status, respectively; λ3 = z/Z describes the deformation in the axial direction, which is denoted by Z and z in the undeformed and deformed status, respectively; and ϕ is the angle of twist per unit deformed length and is related to the shear strain γ by γ = rϕ

(7.155)

We note that if the value of λi (i = m, 2, 3) is greater than one, then it implies stretching; if it is equal to one, then there is no length change; and there is contraction when this value is less than one. Taylor and Quinney [9] found

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

387

that the hoop and radial strains are not equal for a thin-walled tube under combined tension–torsion loading condition. According to Taylor and Quinney, the values of λm and λ2 are the same for the tension only condition but are different and depend on the constitutive equations used for the combined tension–torsion loading condition. It has been shown in Example 7.6 that the physical components of deformation gradient F are

∂r ∂Z r∂θ ∂Z ∂z

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂R r∂θ [F] = ∂R ∂z ∂R

(7.156)

∂Z

Using (7.154), (7.156) reduces to

λ2

[F] = 0 0

λ2 0 = ϕλ3 r 0 λ3

0 r R 0

0

0 λm 0

0 γ λ3 λ3

(7.157)

The last expression of (7.157) is found by considering the mean radius of the tube, where R = Rm , r = rm = λm Rm and γ = rm ϕ. The inverse of the above matrix is

λ−1 2

[F]−1 = 0 0

0

0

λ−1 m

−Rm ϕ

(7.158)

λ−1 3

0

When the material is incompressible, which is a reasonable assumption for metallic materials undergoing large plastic deformation, the Jacobian is J = β2 β3 βm = 1

(7.159)

We now proceed to ﬁnd the relations among the components of Cauchy stress σ, 1st P–K stress T(0) , and 2nd P–K stress . These relations have been previously discussed in Section 4.4.2.1, and the equations are from (4.42) and (4.50) σ = J −1 F · T(0)

and

= T(0) · F−T

(7.160)

For the case of thin-walled tube under axial–torsional loading condition, the stress states of σ, T(0) , and are given by their respective physical

© 2005 by Chapman & Hall/CRC Press

388

Continuum Mechanics and Plasticity

components as

0 [σ ] = 0 0

0 0 τ

0 τ, σ

0 (0) [T ] = 0 0

0 T θθ T zθ

0 T θz , T zz

0 [] = 0 0

0 θθ zθ

0 θz zz (7.161)

in which σ zz = σ is the axial stress which is equal to the axial force divided by 2πrm h; σ θz = σ zθ = τ is the shear stress, which is equal to the torque divided 2 h; σ θθ = 0 due to symmetry and σ rr = 0 due to no surface tractions by 2π rm on both the inner and outer lateral surfaces of the tube. The last condition is an approximation, but it is justiﬁable when the wall is thin. Substituting (7.157) to (7.159) and (7.161) into (7.160), we obtain 0 0 0 [σ ] = 0 λm T θθ + ϕRm λm λ3 T zθ λm T θz + ϕRm λm λ3 T zz 0 λ3 T zθ λ3 T zz 0 0 0 1 0 −τ Rm ϕ (τ − ϕRm λm σ ) [T (0) ] = λm τ σ 0 λ3 λ3 0 0 0 T θz 0 1 T θθ − ϕRm λm T θz [] = λm λ3 T zz 1 zθ zz 0 T − ϕRm λm T λm λ3

(7.162)

(7.163)

(7.164)

The component T zθ , which equals the torque divided by 2π Rm Hrm , and the component T zz , which equals the axial force divided by 2π Rm H, are known quantities from experiment, where Rm is the mean radius of the tube in the undeformed conﬁguration and an approximated rm may be obtained by measuring the deformed outer radius r1 and then subtracting H/2 from it. For convenience, most experimental results in the literatures are presented in terms of the 1st P–K stress components T zz and T zθ . However, this is only an approximation since rm is not measured in most experiments. The current wall-thickness h is very difﬁcult to measure. The other components of T(0) cannot be readily determined experimentally in the case considered. However, they may be expressed in terms of T zz and T zθ . To this end, we obtain, from (7.161) and (7.162), the following relations σ θθ = 0 = λm T θθ + ϕRm λm λ3 T zθ σ

© 2005 by Chapman & Hall/CRC Press

θz

= τ = λm T

θz

+ ϕRm λm λ3 T

zz

(7.165) (7.166)

Advances in Plasticity

389 σ zθ = τ = λ3 T zθ σ

zz

(7.167)

zz

(7.168)

T θθ = −ϕRm λ3 T zθ

(7.169)

= σ = λ3 T

From (7.165), we obtain

and, by substituting (7.167) into (7.166), we have T θz =

1 λ3 T zθ − ϕRm λm λ3 T zz λm

(7.170)

Thus, all components of the 1st P–K stress may be determined. By using (7.167) and (7.168), Cauchy stress components may be calculated. In view of (7.161), the state of Cauchy stress can be completely determined. It is seen that when the axial strain is equal to zero, that is, λ3 = 1, we have σ zθ = T zθ and σ zz = T zz . But if the axial strain is large, then the difference between the two measures can be large. These transformation equations are used in the next section where theoretical predictions of yield surfaces are compared with experimental data. For the axial prestrain only condition, we have λm equaling λ2 [9]. From (7.159), we then obtain the relations among λi as λm = λ2 =

1 λ3

(7.171)

For the torsional prestrain only condition, all values of λi ’s may be approximated by one. This may be estimated by use of experimental results of Wu and Xu [80] for pure torsion of 304 stainless steel. It has been found that for an angle of relative grip rotation of 32.5◦ , ϕ is 12.76 rad/m and the corresponding engineering shear strain is 10.3%, which gives rise to an axial strain ε of 0.23%. Using (7.154), we found that λ3 = 1.0023 which may be approximated by 1 in this case. Since the diameter of the thin-walled tube undergoes a small amount of change during pure torsion, we obtain the following approximated relations among λi , that is, λm ∼ = λ2 ∼ = λ3 ∼ = 1. These relations are used in the next section and are further discussed. 7.6.6.2 Experimental determination of yield surfaces Experiments were conducted, by use of a computer-controlled, axial– torsional, closed-looped, electrohydraulic materials test system. The same batch of annealed 304 stainless steel specimens as in Wu and Yeh [4] was used in this investigation. Detailed information about the material, specimens, strain measurement, and experimental procedures may be found in Wu and Yeh [4] and Wu et al. [24]. We only mention here that initial and

© 2005 by Chapman & Hall/CRC Press

390

Continuum Mechanics and Plasticity 150

Shear stress (MPa)

100

= First P. K. St. = Cauchy St.(th.) = Cauchy St.(ex.) = Second P. K. St.

50

0

–50

–100

–150 350.

450. 550. Axial stress (MPa)

650.

FIGURE 7.28 Subsequent yield surfaces due to tension prestrain determined by various stress measures (From Wu, H.C. et al., J. Appl. Mech., 62, 626, 1995. With permission from ASME).

subsequent yield surfaces were determined for two loading paths. Path (1) in axial loading had an axial prestrain of 20% and path (2) in free-end torsion had a shear prestrain of 20%. After the subsequent yield surface was determined for each loading path, the specimen was removed from the test machine and cut through the cross-section in the middle of the gauge section. By measuring the change of the cross-sectional area, it was found that the reduction of the cross-sectional area was 17% for path (1) and no observable area change was found for path (2). Now the effect of stress measure on the shape, size, and translation of the yield surface is investigated. Figure 7.28 shows the subsequent yield surfaces for path (1). The experimental yield surface (using the 1st P–K stress components) is shown in the middle of the ﬁgure. Also shown in the ﬁgure are the theoretical yield surfaces of the Cauchy stress components determined from (7.161), (7.167), and (7.168) and the 2nd P–K stress components obtained by (7.164). As an independent veriﬁcation, the experimental Cauchy yield surface is also shown in the ﬁgure. The experimental Cauchy stress components were determined based on the measured deformed area. The agreement between the two Cauchy yield surfaces is generally good. However, it may be observed from the ﬁgure that the amount of axial strain affects the size of the Cauchy yield surface. In fact, from (7.167) and (7.168), σ = λ3 T zz and τ = λ3 T zθ and the Cauchy yield surface is an isotropic expansion of

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

391

the 1st P–K yield surface with λ3 being the factor of expansion. For an axial prestrain of 20%, the size of the Cauchy yield surface is about 20% larger than that of the corresponding 1st P–K yield surface. We also note that the translation (the back stress) of the former yield surface is 20% more than that of the latter. In the case of the 2nd P–K stress, we have zθ ∼ = (T zθ /λm ) and zz zz ∼ = (T /λ3 ) from (7.164) for ϕ approximately equal to zero (ϕ is zero during axial prestrain and is very small and negligible during the probing of yield surface). The 2nd P–K yield surface is about 9.5% larger than that of the 1st P–K yield surface in the shear direction but is about 17% smaller in the axial direction. The back stress of the former is 17% less than that of the latter. These results have suggested that the evolution rules for both isotropic and kinematic hardening are stress measure dependent. Figure 7.29 shows the subsequent yield surfaces determined by each stress measure for path (2). Due to no observable change in the cross-sectional area, the Cauchy stress components σ and τ are almost identical to the 1st P–K stress components T zz and T zθ from (7.167) and (7.168). Therefore, the Cauchy and the 1st P–K yield surfaces are indistinguishable in the ﬁgure. However, the components of the 2nd P–K stress are different from those of the Cauchy stress. Using the approximation that all λ’s are equal to 1, (7.164) reduces to zθ ∼ = T zθ − ϕRm T zz and zz ∼ = T zz , that is, the component zθ depends

800

Shear Stress (MPa)

= First P.K. and Cauchy St. (th. and ex.) = Second P.K. St.

500

400

300 –150

0.0 Axial Stress (MPa)

150

FIGURE 7.29 Subsequent yield surfaces due to torsion prestrain determined by various stress measures (From Wu, H.C. et al., J. Appl. Mech., 62, 626, 1995. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

392

Continuum Mechanics and Plasticity

on the twist angle per unit length ϕ. This leads to a rotation of the 2nd P–K surface, with the angle of rotation increasing with the shear strain. It also leads to a further distortion of the 2nd P–K surface in that the yield surface is not symmetric with respect to the shear stress axis. These results complicate the hardening rule associated with the 2nd P–K yield surface. In the aforementioned example, the theoretical results in the case of pretorsion are calculated based on the approximation that all λ’s are equal to 1. Without this approximation, the axial strain exists but is very small. It is less than 0.3% for a prestrain in torsion of 20%. In this case, 1.003 > λ3 > 1 and, from Wu et al. [74] where the circumferential strain was investigated, we obtain 0.9973 < λm < 1. Thus, the effect of this approximation is very small. Also, we emphasize that the rotation and distortion of the 2nd P–K surface is independent of this approximation. EXAMPLE 7.8 Transform the Mises yield criterion in the Cauchy stress space into the stress spaces of the 1st and 2nd P–K stresses.

Solution The Mises yield surface in the Cauchy stress space is (σ − ασ )2 + 3(τ − ατ )2 = k 2

(a)

where ασ and ατ are, respectively, the axial and shear components of the back stress. k is the shear yield stress and is assumed to be constant in this discussion. Using (7.167) and (7.168), (a) is transformed into T

zz

ασ − λ3

2

+3 T

zθ

ατ − λ3

2

=

k λ3

2 (b)

Using (7.164), (b) is further transformed into an equation in the zθ versus zz stress space. In the case of axial prestrain only, ϕ ∼ = 0 and ατ = 0; and using (7.171), the yield function in the zθ versus zz stress space may be written as (zz − (ασ /λ23 ))2 (k/λ23 )

+

(zθ )2 =1 √ (k/ 3λ3 )2

(c)

By comparing equations (a), (b), and (c), we see that the semimajor axes (in the axial stress direction) of the ellipses are k for the Cauchy yield surface, k/λ3 for the 1st P–K surface, and k/λ23 for the 2nd P–K surface. The semiminor axes √ √ √ (in the shear stress direction) are, respectively, k/ 3, k/ 3λ3 , and k/ 3λ3 . The back stress for the three yield surfaces are respectively ασ , ασ /λ3 , and ασ /λ23 . It is seen that the size, shape, and the back stress of the yield surfaces are all inﬂuenced by the deformation of the material element when different stress measures are used.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

393

In the case of torsion only prestrain, ασ = 0. If we use the approximation that all λ’s are one, then the yield surface in the 2nd P–K stress space is governed by the equation (zz )2 + 3[(zθ + ϕRm zz ) − ατ ]2 = k 2

(d)

This equation contains a 6ϕRm zθ zz term, and a rotation in the ellipse will occur. 7.6.6.3 Discussions We have seen from the previous section that the size, shape, and position of the subsequent yield surfaces depend greatly on the stress measure used to deﬁne the yield surface. The different positions of the yield surfaces in the stress space correspond to different degrees of kinematic hardening. We have seen that the hardening rules (isotropic and kinematic hardening) depend greatly on the deﬁnition of stress. The 2nd P–K stress which is often used in the computational mechanics can lead to a yield surface which rotates due to a shear prestrain, while no rotations have been found for this proportional path using the Cauchy stress or the 1st P–K stress. Therefore, the yield surface and the hardening rule should be paired. They vary with the deﬁnition of stress. The yield surface deﬁned by the 2nd P–K stress is independent of imposed rigid-body rotation. In order for the Cauchy yield surface (yield surface deﬁned by the Cauchy stress) to be independent of rigid-body rotation, the yield function has to be a function of stress invariants. The yield surface will be discussed further in Chapter 11 using the true stress in the convected coordinate system. The contravariant components of the true stress do not change with imposed rigid-body rotation.

References 1. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech., 23, 517, 1971. 2. Valanis, K.C., Fundamental consequences of a new intrinsic time measureplasticity as a limit of the endochronic theory, Arch. Mech., 32, 171, 1980. 3. Ohashi, Y. and Tokuda, M., Precise measurement of plastic behavior of mild steel tubular specimens subjected to combined torsion and axial force, J. Mech. Phys. Solids, 21, 214, 1973. 4. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 5. Phillips, A. and Lu, W.Y., An experimental investigation of yield surfaces and loading surfaces of pure aluminum with stress-controlled and strain-controlled paths of loading, J. Eng. Mater. Technol., 106, 349, 1984.

© 2005 by Chapman & Hall/CRC Press

394

Continuum Mechanics and Plasticity

6. Ivey, H.J., Plastic stress–strain relations and yield surfaces for aluminum alloys, J. Mech. Eng. Sci., 3, 15, 1961. 7. Wu, H.C. and Yang, C.C., Investigation of the one-dimensional endochronic constitutive equation for metals by the Rivlin test, J. Eng. Mater. Technol., 106, 264, 1984. 8. Ellis, J.R., Robinson, D.N., and Pugh, C.E., Time dependence in biaxial yield of type 316 stainless steel at room temperature, J. Eng. Mater. Technol., 105, 250, 1983. 9. Taylor, G. I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc. A, 230, 323, 1931. 10. Naghdi, P.M., Essenburg, F., and Koff, W., Experimental study of initial and subsequent yield surface in plasticity, J. Appl. Mech., 201, 1958. 11. McComb, H.G. Jr., Some experiments concerning subsequent yield surface in plasticity, NASA TN D-396, 1960. 12. Mair, W.M. and Pugh, H.L.D., Effect of prestrain on yield surfaces in copper, J. Mech. Eng. Sci., 6, 150, 1964. 13. Bertsch, P.K. and Findley, W.N., An experimental study of subsequent yield surfaces-corners, normality, Bauschinger effect and allied effects, Proc. 4th U.S. Nat. Cong. Appl. Mech., 893, 1962. 14. Phillips, A. and Moon, H., An experimental investigation concerning yield surfaces and loading surfaces, Acta Mech., 27, 91, 1977. 15. Shiratori, E., Ikegami, K., Yoshida, F., Kaneko, K., and Koike, S., The subsequent yield surface after preloading under combined axial load and torsion, Bull. JSME, 19, 877, 1976. 16. Ishikawa, H., Subsequent yield surface probed from its current center, Int. J. Plasticity, 13, 533, 1997. 17. Lode, W., Versuche über den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle, Eisen, Kupfer und Nickel, Z. Phys., 36, 913, 1926. 18. Hu, L.W. and Bratt, J.F., Effect of tensile plastic deformation on yield criterion, J. Appl. Mech., 25, 411, 1958. 19. Szczepinski, W., On the effect of plastic deformation on yield criterion, Arch. Mech., 15, 276, 1963. 20. Szczepinski, W. and Miastkowski, J., An experimental study of the effect of the prestraining history on the yield surfaces of an aluminum alloy, J. Mech. Phys. Solids, 16, 153, 1968. 21. Shiratori, E. and Ikegami, K., Experimental study of the subsequent yield surface by using cross-shaped specimens, J. Mech. Phys. Solids, 16, 373, 1968. 22. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Structures, 8, 463, 1972. 23. Helling, D.E., Miller, A.K., and Stout, M.G., An experimental investigation of the yield loci of 1100-0 aluminum, 70 : 30 brass, and an overaged 2024 aluminum alloy after various prestrains. J. Eng. Mater. Technol., 108, 313, 1986. 24. Wu, H.C., Lu, J.K., and Pan, W.F., Some observations on yield surfaces for 304 stainless steel at large strain, J. Appl. Mech., 62, 626, 1995. 25. Wu, H.C., Effect of loading-path on the evolution of yield surface for anisotropic metals subjected to large pre-strain, Int. J. Plasticity, 19, 1773, 2003. 26. Wu, H.C. and Xu, Z., An axial–torsional extensometer for ﬁnite deformation, J. Eng. Mater. Technol., 112, 330, 1990. 27. Phillips, A., A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity, 2, 315, 1986.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

395

28. Wu, H.C., Viscoplasticity Under Complex States of Stress, Ph.D. thesis submitted to Yale University, New Haven, CT, 1970. 29. Phillips, A. and Wu, H.C., A theory of viscoplasticity, Int. J. Solids Struct., 9, 15, 1973. 30. Phillips, A., Experimental plasticity. Some thoughts on its present status and possible future trends, in Problems of Plasticity, Sawczuk, A. Ed., Nordhoff International Publishing Leyden, 1974, 193. 31. Krempl, E., Models of viscoplasticity. Some comments on equilibrium (back) stress and drag stress, Acta Mech., 69, 25, 1987. 32. Phillips, A., Liu, K., and Justusson, W.J., An experimental investigation of yield surfaces at elevated temperatures, Acta Mech., 14, 119, 1972. 33. Phillips, A. and Kasper, R., On the foundations of thermoplasticity — an experimental investigation, J. Appl. Mech., 40, 891, 1973. 34. Phillips, A., Tang, J.-L., and Ricciuti, M., Some new observations on yield surfaces, Acta Mech., 20, 23, 1974. 35. Phillips, A. and Kawahara, W.A., The effect of thermal loading on the yield surface of aluminum, An experimental investigation, Acta Mech., 50, 249, 1984. 36. Ohashi, Y., Kawashima, K., and Yokochi, T., Anisotropy due to plastic deformation of initially isotropic mild steel and its analytical formulation, J. Mech. Phys. Solids, 23, 277, 1975. 37. Phillips, A. and Kaechele, L., Combined stress tests in plasticity, J. Appl. Mech., 23, 43, 1956. 38. Khan, A.S. and Wang, X., On non-proportional inﬁnitesimal plastic deformation after ﬁnite plastic prestressing and partial unloading, J. Mech. Phys. Solids, 36, 519, 1988. 39. Mroz, Z., On the description of anisotropic workhardening, J. Mech. Phys. Solids, 15, 163, 1967. 40. Masing, G., Wiss. Veröff. Siemens-Konzern, III Band, 1927. 41. Dafalias, Y.F. and Popov, E.P., A model of nonlinear hardening materials for complex loading, Acta Mech., 21, 173, 1975. 42. Dafalias, Y.F. and Popov, E.P., Plastic internal variables formalism of cyclic plasticity, J. Appl. Mech., 98, 645, 1976. 43. Ilyushin, A.A., On the relation between stresses and small strains in continuum mechanics, Prikl. Mat. Mekh., 18, 641, 1954 (in Russian). 44. Ilyushin, A.A., Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 1963 (in Russian). 45. Lensky, V.S., Analysis of plastic behavior of metals under complex loading, in Proc. 2nd Symposium on Naval Struc. Mech., Lee, E.H. and Symonds, P.S., Eds., Brown University, Pergamon Press, 1960, 259. 46. Ohashi, Y., Tokuda, M., and Tanaka, Y., Precise experimental results on plastic behavior of brass under complex loading, Bull. De L’Acad. Polon. Des Sci., Ser. Sciences Tech., 26, 261, 1978. 47. Ohashi, Y., Kurita, Y., Suzuki, T., and Tokuda, M., Effect of curvature of the strain trajectory on the plastic behavior of brass, J. Mech. Phys. Solids, 29, 69, 1981. 48. Pipkin, A.C. and Rivlin, R.S., Mechanics of rate-independent materials, J. Appl. Math. Phys. (ZAMP), 16, 313, 1965. 49. Zhou, Z.-D., Zhao, S.-X., and Kuang, Z.-B., An integral elasto-plastic constitutive theory, Int. J. Plasticity, 19, 1377, 2003. 50. Ilyushin, A.A., in Problems in the Theory of Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 1961, 3 (in Russian).

© 2005 by Chapman & Hall/CRC Press

396

Continuum Mechanics and Plasticity

51. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 52. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strainpath, Int. J. Non-Linear Mech., 20, 41, 1985. 53. Wu, H.C., Aboutorabi, M.R., and Chen, P.C.T., Cyclic torsion of a circular cylinder and its residual stress distribution, J. Eng. Mater. Technol., 107, 48, 1985. 54. Wu, H.C. and Yeh, W.C., Some considerations in the endochronic description of anisotropic hardening, Acta Mech., 69, 59, 1987. 55. Wu, H.C. and Ho, C.C., An investigation of transient creep by means of endochronic viscoplasticity and experiment, J. Eng. Mater. Technol., 117, 260, 1995. 56. Green, A.E. and Naghdi, P.M., Ageneral theory of an elastic–plastic continuum, Arch. Rat. Mech. Anal., 18, 251, 1965. 57. Lee, E.H., Elastic–plastic deformations at ﬁnite strains, J. Appl. Mech., 36, 1, 1969. 58. Dafalias, Y.F., A missing link in the macroscopic constitutive formulation of large plastic deformations, in Plasticity Today, Sawczuk, A. and Bianchi, G., Eds., Elsevier Applied Science, London, 1983, 135. 59. Mandel, J., Plasticité classique et viscoplasticité, CISM Courses and Lectures 97, Springer, New York, 1971. 60. Montheillet, F., Cohen, M., and Jonas, J.J., Axial stresses and texture development during the torsion testing of Al, Cu and A-Fe, Acta Metall., 32, 2077, 1984. 61. Stout, M.G. and O’Rourke, J.A., Experimental deformation textures of OFE copper and 70 : 30 brass from wire drawing, compression and torsion, Metall. Trans. 20A, 125, 1989. 62. Toth, L.S., Jonas, J.J., Daniel, D., and Bailey, J.A., Texture development and length changes in copper bars subjected to free-end torsion, Text. Microstruct. 19, 245, 1992. 63. Wang, P.T., Panchanadeeswaran, S., and Wu, H.C., Comparison of ﬂow stress and texture for P0815 cast aluminum deformed in compression and in torsion. Alcoa Technical Center Research Report, Alcoa Center, Pa., U.S.A., 1995. 64. Dafalias, Y.F., Plastic spin: necessity or redundancy?, Int. J. Plasticity, 14, 909, 1998. 65. Kratochvil, J., Finite strain theory of crystalline elastic–inelastic materials, J. Appl. Phys., 42, 1104, 1971. 66. Wang, C.C., A new representation theorem for isotropic functions: an answer to Professor G.F. Smith’s criticism of my paper on representations for isotropic functions, Arch. Rat. Mech. Anal., 36, 166, 1970. 67. Loret, B., On the effects of plastic rotation in the ﬁnite deformation of anisotropic elastoplastic materials, Mech. Mater., 2, 287, 1983. 68. Dafalias, Y.F., The plastic spin, J. Appl. Mech., 52, 865, 1985. 69. Dienes, J.K., On the analysis of rotation and stress rate in deforming bodies, Acta Mech., 32, 217, 1979. 70. Nagtegall, J.C. and de Jong, J.E., Some aspects of non-isotropic workhardening in ﬁnite strain plasticity, in Proc. Workshop on Plasticity of Metals at Finite Strain:

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

71. 72. 73. 74. 75. 76.

77. 78. 79. 80.

397

Theory, Experiment and Computation, Lee, E.H. and Mallet, R.L., Eds., Stanford University, 1981, 65. Cotter, B.A. and Rivlin, R.S., Tensors associated with time-dependent stress, Quart. Appl. Math., 18, 177, 1955. Oldroyd, J.G., On the formulation of rheological equations of state, Proc. Roy. Soc., A, 200, 523, 1950. Aifantis, E.C., The physics of plastic deformation, Int. J. Plasticity, 3, 221, 1987. Wu, H.C., Xu, Z., and Wang, P.T., Torsion test of aluminum in the large strain range, Int. J. Plasticity, 13, 873, 1998. Truesdell, C., The simplest rate theory of pure elasticity, Comm. Pure Appl. Math., 8, 123, 1955. Khan, A.S. and Wang, X., An experimental study of large ﬁnite plastic deformation in annealed 1100 aluminum during proportional and nonproportional biaxial compression, Int. J. Plasticity, 6, 485, 1990. Lee, E.H., Mallet, R.L., and Wertheimer, T.B., Stress analysis of anisotropic hardening in ﬁnite-deformation plasticity, J. Appl. Mech., 50, 554, 1983. Wu, H.C., On ﬁnite plastic deformation of anisotropic metallic materials, Int. J. Plasticity, 19, 91, 2003. Wu, H.C., Effect of loading-path on the evolution of yield surface for anisotropic metals subjected to large pre-strain, Int. J. Plasticity, 19, 1773, 2003. Wu, H.C. and Xu, Z., An experimental investigation of the axial effect during torsion, in Advances in Constitutive Laws for Engineering Materials, Fan, J. and Murakami, S., Eds., Int. Academic Publishers, Pergamon Press, Beijing, 1989, 232.

Problems (1) Write a report about additional experimental evidence showing the normality of the plastic strain increment to the subsequent yield surface. (2) Write a report about Ilyushin’s isotropy postulate. (3) Referring to Figure 7.18 in a stress-controlled loading problem, how do surfaces fA , fB , and fC move when the stress point follows path PQ? (4) Derive (7.97) from (7.95). (5) In simple shear problem using Cotter–Rivlin stress rate, show that the solution is given by (7.107) for hypoelastic materials. (6) In simple shear problem using Truesdell’s stress rate, show that the solution is given by (7.110) for hypoelastic materials. (7) In the problem of rectangular metal block discussed in Example 7.3, if µ = 26 GPa and λ = 33 GPa, plot the σx versus Dx dt and σz versus Dx dt curves. In addition, plot Dy as a function of Dx and discuss the effect of h on the results. (8) Use the Jaumann rate to investigate and plot the loading–unloading curve of simple shearing. The material is rigid-plastic with linear kinematic hardening.

© 2005 by Chapman & Hall/CRC Press

398

Continuum Mechanics and Plasticity During loading, the simple shear deformation is governed by x1 = X1 + 2ωtX2 ,

x2 = X2 ,

x3 = X3

and its displacement ﬁeld is u1 = 2ωtX2 ,

u2 = u3 = 0,

ω = const

The unloading starts at t* and the displacement ﬁeld during unloading is u1 = [2ωt ∗ −2ω(t − t∗)]x2 = 2ω(2t ∗ −t)x2 ,

u2 = u3 = 0,

for t > t ∗ .

(9) Show that (7.101) may be derived from (7.100). (10) Solve Problem (8) using the Dafalias rate. (11) Solve Problem (8) using Lee’s rate. (12) Find the physical components of deformation gradient F in the spherical coordinate system. (13) In an uniaxial stress test, the following data have been recorded for the axial stress–strain curve: (plastic strain, stress (MPa))={(0, 100), (0.005, 289.59), (0.01, 336.82), (0.02, 369.03), (0.04, 397.35), (0.06, 420.78), (0.1, 458.86), (0.14, 489.12), (0.2, 526.71)}. The stress has been calculated based on the undeformed cross-sectional area. Plot the equivalent stress versus equivalent plastic strain curves using the Cauchy stress, the 1st P–K stress and the 2nd P–K stress as stress measure, respectively. (14) In a torsion test of thin-walled tubular specimen, the following data have been recorded for the shear stress–strain curve: ( plastic shear strain, shear stress (MPa))={(0, 100), (0.005, 273.36), (0.01, 309.48), (0.02, 334.87), (0.04, 362.20), (0.06, 387.10), (0.1, 428.59), (0.14, 469.60), (0.2, 521.34)}. The stress has been calculated based on the undeformed cross-sectional area. Plot the equivalent stress versus equivalent plastic strain curves using the Cauchy stress, the 1st P–K stress and the 2nd P–K stress as stress measure, respectively. Compare these curves with those obtained in Problem (13).

© 2005 by Chapman & Hall/CRC Press

8 Internal Variable Theory of Thermo-Mechanical Behaviors and Endochronic Theory of Plasticity

8.1

Introduction

There are several approaches to irreversible thermodynamics. One of them, the internal variable theory, is widely used in recent literature of mechanics of solids. In this chapter, the concept and equations of the internal variable theory of irreversible thermodynamics, which are used to describe the thermo-mechanical behavior of materials are ﬁrst discussed. Based on this thermodynamic foundation, it is shown how a theory of plasticity, known as the endochronic theory, can be developed. Applications of the endochronic theory to metals, geotechnical materials, and damage mechanics are then discussed in this chapter and Chapter 9. The theory of thermodynamics that is presented owes much to the work of Valanis [1–4]. A summary of Valanis’ works on the internal variable theory of thermodynamics is nicely presented in [5], although it does not contain recent works on the gradient theory. The gradient theory is outside scope of this book, but readers are referred to [4] for further reading. The endochronic theory of plasticity was developed by Valanis [6,7] and this author had the privilege of learning the theory directly from Professor Valanis and has been heavily involved in the further development and veriﬁcation of the theory. Other researchers have also made signiﬁcant contributions to the theory.

8.2 8.2.1

Concepts and Terminologies of Thermodynamics The First Law of Thermodynamics

Irreversible thermodynamics is also known as the nonequilibrium thermodynamics. It is needed because we are dealing with an irreversible system, which is a material region R. A reversible system exists only in an ideal gas or an ideal elastic material. It is assumed that the system possesses an internal 399

© 2005 by Chapman & Hall/CRC Press

400

Continuum Mechanics and Plasticity

energy E with density ε (read also Section 4.3.3). Readers are referred to Callen [8] for measurability of internal energy. The mechanical variables are stress, deformation, and mass. In addition, temperature is a variable. Amechanical process is a process during which energy (in the absence of heat supply, e.g., heat sources) is transmitted to the system through an adiabatic boundary by motion of the boundary and/or application of long-range forces. The adiabatic boundary is a boundary through which no heat can ﬂow. This type of energy is called work, denoted by W . A thermal process is a process during which energy ﬂows through the boundary of the system and/or is supplied to its interior while its boundary remains stationary and there are no long range (gravitational, say) forces acting. This type of energy is called heat, denoted by Q. Conduction is a process during which energy is supplied to the system by heat ﬂow through its boundary. A boundary and/or a process which is not adiabatic will be called diathermal. Conduction is a diathermal process. The ﬁrst law of thermodynamics is a statement of the conservation of energy discussed in Section 4.3.3. In the local form, which applies to an inﬁnitesimal neighborhood of a material region, the energy balance equation is from (4.34) ρ ε˙ = σki vi,k − hi,i + ρ q˙

(8.1)

where ρ is the current mass density; hi is the heat ﬂux vector, in which the direction of the vector is the direction of the heat ﬂow; q is the internal energy supply per unit mass by radiation or “other sources” such as electric conductors; and the dot denotes the material differentiation. We note that |hi | is the amount of energy ﬂow per unit area normal to the direction of heat ﬂow per unit time. Referring to the undeformed conﬁguration, the energy balance equation is from (4.68) ε˙ =

1 ∂hR 1 1 ˙ RS E˙ RS − + q˙ = RS E˙ RS + Q ρ0 ρ0 ∂XR ρ0

˙ =− with Q

1 ∂hR + q˙ ρ0 ∂XR (8.2)

˙ is the rate of heat supply per unit volume (conduction and radiation). where Q

8.2.2

State Variables, State Functions, and the Second Law of Thermodynamics

The change of internal energy may be accomplished through (1) a purely thermal process (radiation, heat conduction, etc.), which changes the temperature of the system, or (2) an adiabatic process, that is, work, which changes the position of the boundary and causes the system to deform. Thus, strain and temperature are measures of the internal energy of the system. They are called state variables, since they serve to deﬁne the state of the system. Internal

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

401

energy is a state function, which is a function of state variables. The thermodynamic state of the system is represented by the state functions. One of the main tasks of thermodynamics is to establish those quantities that are state functions and those that are not and to establish useful relationships between state functions. In a reversible system, the internal energy and stress are state functions written as ε = ε(ERS , T)

and

RS = RS (EPQ , T)

(8.3)

where ERS is the strain and T the temperature. The fundamental issue is that the increment of heat supply dQ is not an exact differential. The meaning of this statement is not obvious without further clariﬁcations and deﬁnitions. A reversible system is said to undergo a reversible process if its thermodynamic state is being changed under adiabatic conditions. It is an irreversible process when the process is diathermal. In this case, dQ is not an exact differential, where dQ = 0 following a closed contour in the (ERS , T) space. From (8.2), we have

dε =

1 RS dERS + ρ0

dQ

(8.4)

The integral on the left-hand side is zero because ε is a state function given by (8.3). The ﬁrst integral on the right-hand side represents the amount of work done on the system, which in general is not zero when the path of integration involves thermal processes. The statement may be better understood by examining the Carnot cycle, which is a reversible cycle for ideal gas carried out with the piston–cylinder arrangement. The Carnot cycle goes through two reversible isothermal processes connected by two reversible adiabatic processes and the work done is not zero. Thus, from (8.4) dQ = 0

(8.5)

Hence, dQ is not an exact differential and we cannot write Q = Q(ERS , T). However, in the case of an ideal gas, dQ/T is an exact differential in the sense that dQ/T = 0. Therefore, deriving dS = dQ/T, we ﬁnd that dS is an exact differential. Thus, in the case of a gas dQ = T dS(ERS , T), where S = S(ERS , T), which is a state function known as entropy. An important contribution by Valanis [2] is the proof of the existence of entropy in irreversible systems, establishing the entropy as a state function. We now consider the reversible system and leave the irreversible system for later discussion. In the case of the reversible system, the energy equation (8.2) is written as dε −

1 RS dERS = dQ = θ(ERS , T) dη(ERS , T) ρ0

© 2005 by Chapman & Hall/CRC Press

(8.6)

402

Continuum Mechanics and Plasticity

where θ is the integrating factor; η is the speciﬁc entropy, and (8.6) is integrable so that η is a state function, that is, η = η(ERS , T). The equation dη = gQ/θ is also known as the second law of thermodynamics. The factor θ(ERS , T) has the signiﬁcance of empirical temperature. We note that entropy is dimensionless, and temperature has the dimensions of energy [8]. The units of temperature depend on the nature of the thermometric substance used. Temperature measured by a mercury thermometer is not exactly the same as that given by an electrical resistance thermometer except at their common points. Degree Kelvin is the absolute temperature. Using (8.3), (8.6) is ∂ε ∂ε 1 dERS + dT − RS dERS = θ ∂ERS ∂T ρ0

∂η ∂η dERS + dT ∂ERS ∂T

(8.7)

Since ERS and T can be independently varied and dERS and dT are arbitrary, the following are obtained 1 ∂ε ∂η RS = −θ ρ0 ∂ERS T ∂ERS T

and

∂ε ∂η =θ ∂T ∂T

(8.8)

Since θ = θ (ERS , T), we can express the state functions as ε = ε(θ , ERS ) and η = η(θ , ERS ). Using the chain rule of differentiation, we have ∂ε ∂ε = ∂T ∂θ ERS ∂ε ∂ERS T ∂η ∂ERS T

∂θ ∂η ∂η ∂θ , = ∂T ERS ∂T ∂θ ERS ∂T ERS ∂θ ∂ε ∂ε = + ∂θ ERS ∂ERS T ∂ERS θ ∂θ ∂η ∂η = + ∂θ ERS ∂ERS T ∂ERS θ

(8.9)

By substituting (8.9) into (8.8), we obtain ∂ε ∂η 1 RS = − θ ∂ERS θ ∂ERS θ ρ0

and

∂ε ∂η =θ ∂θ ∂θ

(8.10)

This equation has the same form as (8.8). It shows that the form of the equation is independent of the temperature scale used, and the state functions can be expressed as ε = ε(ERS , θ ) and RS = RS (EPQ , θ). We now introduce a new state function, deﬁned by (ERS , θ) = ε − θη, which is known as the Helmholtz free energy. Differentiating , we have ∂ ∂ε ∂η = −θ ∂ERS θ ∂ERS θ ∂ERS θ

© 2005 by Chapman & Hall/CRC Press

and

∂ ∂ε ∂η = −θ − η. ∂θ ∂θ ∂θ

Internal Variable Theory and Endochronic Theory

403

We then substitute these expressions into (8.10) to obtain 1 ∂ RS = ρ0 ∂ERS

and

η=−

∂ ∂θ

(8.11)

These are the constitutive equations for reversible systems.

8.3 8.3.1

Thermodynamics of Internal State Variables Irreversible Systems

In some systems, the state functions are not uniquely determined by the state variables ERS and T of the system. For instance, in materials undergoing plastic deformation, the current state of stress will depend on the whole history of the deformation. In the case of uniaxial loading–unloading at constant temperature, the stress, which is a state function, is not uniquely determined by the strain E11 , as shown in Figure 8.1. Both points A and B have the same strain, but the states of the internal structure of the material are different at the two points. It is therefore necessary to introduce other macroscopic parameters, additional to strain and temperature, which are representative of the internal structure of the material. Another example that shows the inadequacy of the state of strain in predicting the state of stress is given in Figure 8.2. We represent the unknown material to be tested at constant temperature by a black box. Within the black box there are the spring and dashpot elements with elastic moduli E1 and E2 for the springs. If we do not know the internal structure of the black box and test it macroscopically, the state of stress σ cannot be described uniquely in terms of the state of strain of the black box. Other parameters (internal variables) will have to be used in order to determine the stress. However, if we Π11

A

B E11

FIGURE 8.1 Stress not uniquely determined by strain.

© 2005 by Chapman & Hall/CRC Press

404

Continuum Mechanics and Plasticity Black Box E1

E2

Dashpot

FIGURE 8.2 Test of black box.

open the black box and know the internal structure and constitution of the black box, that is, we know the properties and arrangement of the springs and the dashpot, then we know that the overall strain of the black box is the same as the strain of spring 1, and, if we also know the strain of the dashpot as a function of time, we are able to describe the stress uniquely. The strain of the dashpot is the internal variable needed to uniquely describe the stress. For this example, the stress is a function of the overall strain and the strain of the dashpot. In the materials modeling, n parameters may be needed to uniquely deﬁne the stress state. These parameters are called internal (state) variables and are denoted by qr , where r = 1, . . . , n. Internal state variables are called internal coordinates by some authors. They can be scalars, but, generally, they are tensors. It is assumed that sufﬁcient additional state variables (not all observable) can always be found to describe the thermodynamic state of an irreversible system. As previously mentioned, the internal state variables are the macroscopic representations of microscopic effects that have physical meanings. They may represent observed effects due to slips at the crystallographic level or represent dislocations, etc. Owing to the difference in scale, these effects may not be directly observable at the macroscopic scale and are represented by the internal variables. In the mechanics literature, some investigators have been able to identify the physical meanings of their internal variables at the microscopic level. In that case, they are able to use the evolution rules for those physical quantities obtained from experiments at the microscopic level. Mathematically speaking, the internal variables are state variables and the state functions are deﬁned in terms of the state variables. As long as the evolution equations are provided for the state variables, the problem can be solved without assigning physical meanings to the internal variables. For an irreversible system, the state functions are functions of strain, temperature, and n numbers of internal variables, and they are represented by ε = ε(ERS , θ , qrRS ), r = 1, . . . , n

© 2005 by Chapman & Hall/CRC Press

η = η(ERS , θ , qrRS ),

RS = RS (EPQ , θ , qrRS ), (8.12)

Internal Variable Theory and Endochronic Theory

405

Valanis [2] proved the existence of an entropy function η and that the Pfafﬁan form (8.6) of the ﬁrst law of thermodynamics is integrable even for irreversible systems, and thus the entropy is a state function. In an earlier effort, Valanis showed that the constitutive equations for irreversible systems are 1 ∂ε ∂η RS = −θ ρ0 ∂ERS θ,qr ∂ERS θ,qr PQ

and

PQ

∂ε ∂η =θ ∂θ EPQ ,qr ∂θ EPQ ,qr PQ

PQ

(8.13) Valanis [2] assumed that the system behaves reversibly when qrRS are constants and dqrRS = 0 for all r. The derivation from (8.6) to (8.10) can then be used to establish (8.13) for irreversible systems. By using the Helmholtz free energy = ε − ηθ, where = ψ(ERS , θ , qrRS ), (8.13) is further written as 1 ∂ RS = ρ0 ∂ERS

and

η=−

∂ ∂θ

(8.14)

These are powerful results and were independently obtained by Valanis [1] and Coleman and Gurtin [9].

8.3.2

The Clausius–Duhem Inequality

By putting ε = + ηθ into the ﬁrst law of thermodynamics (8.6), we have d + η dθ + θ dη −

1 RS dERS = dQ ρ0

(8.15)

or ∂ ∂ ∂ 1 dERS + dθ + r dqrRS + η dθ + θ dη − RS dERS = dQ ∂ERS ∂θ ∂qRS ρ0 (8.16) Using (8.14), (8.16) is reduced to θ dη +

∂ dqr = dQ ∂qrRS RS

(8.17)

The second term on the left-hand side of (8.17) is absent in a reversible system. In the rate form, (8.17) may be rewritten as ∂ θ η˙ + r ∂qRS E

PQ ,θ

© 2005 by Chapman & Hall/CRC Press

˙ q˙ rRS = θ η˙ + E

PQ,θ

˙ =Q

(8.18)

406

Continuum Mechanics and Plasticity

˙ EPQ ,θ = (∂/∂qr )|EPQ ,θ q˙ r is the rate of change of the Helmholtz The term | RS RS free energy under constant strain and temperature. We now invoke the Kelvin postulate which states that the free energy cannot increase if the strain and the temperature are kept constant, [5]. The postulate is thus written in the mathematical form as ˙ EPQ ,θ ≤ 0 |

(8.19)

˙ EPQ ,θ θ γ˙ ≡ −|

(8.20)

If we deﬁne

then, from (8.19) and (8.20), we obtain γ˙ ≥ 0

(8.21)

where γ˙ is known as the entropy production. Substituting (8.20) into (8.18), we have η˙ =

˙ Q + γ˙ θ

(8.22)

˙ Q θ

(8.23)

which results in η˙ ≥

This inequality is known as the Clausius–Duhem inequality, and the equality holds only for reversible systems. Using (8.22), (8.18) may be written as ˙ + θ γ˙ ) + (Q

∂ r ˙ q˙ = Q ∂qrRS RS

(8.24)

which reduces to θ γ˙ = −

∂ r q˙ ≥ 0 ∂qrRS RS

(8.25)

This is an alternate form for the Clausius–Duhem inequality.

8.3.3

The Helmholtz Formulation of Thermo-Mechanical Behavior

Most of the discussions in the previous section belong to the Helmholtz formulation. We summarize the equations of this formulation here for later reference.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

407

First law of thermodynamics: ε˙ =

1 1 ∂hR RS E˙ RS − + q˙ ρ0 ρ0 ∂XR

(8.26)

Clausius–Duhem (rate of dissipation) inequality: −

∂ r q˙ ≥ 0 ∂qrRS RS

(8.27)

Heat conduction equation: hR = hR (EPQ , θ , θ,P , qrPQ )

(8.28)

where θ,R is the temperature gradient. Equation (8.28) is a generalized form of Fourier’s law of heat conduction, which states that the heat ﬂux vector is proportional to the temperature gradient θ,R . The state functions are = (ERS , θ , qrRS ), η = η(ERS , θ , qrRS ),

ε = ε(ERS , θ , qrRS ) RS = RS (EPQ , θ , qrPQ )

(8.29)

The relations between state functions are RS = ρ0

∂ , ∂ERS

η=−

∂ ∂θ

(8.30)

These relations apply to all materials irrespective of their constitution. The internal state variables qrRS represent the constitutive nature of the material. These internal variables distinguish one material from the other. In an elastic material, qrRS = 0; whereas in a viscoelastic material, qrRS = 0, and the change of qrRS is governed by a set of evolution equations for qrRS . From (8.27), the rate of change q˙ rRS should be related to ∂/∂qrRS so that the inequality is not violated. The simplest relation between the two quantities is expressed in terms of a functional relationship so that q˙ rRS

=

r fRS

∂ ∂qrPQ

r = fRS (EPQ , θ , qrPQ )

where r = 1, . . . , n

(8.31)

The last expression in (8.31) is obtained due to = (EPQ , θ , qrPQ ). The evolution equations for qrRS of a material undergoing plastic deformation will be discussed later in conjunction with the endochronic theory of plasticity.

© 2005 by Chapman & Hall/CRC Press

408

Continuum Mechanics and Plasticity

r , the expressions for Knowing , h,R , and fRS RS and η can be obtained r are subject to the constraints from (8.30). The forms of hR and fRS

−

∂ r q˙ ≥ 0 ∂qrRS RS

and

hR θ,R ≤ 0

(8.32)

The second inequality of (8.32) describes the nature of heat conduction. Heat ﬂows from high to low temperature. In the Helmholtz formulation, there are 22 + n equations. They are listed below with the number of equations shown at the end of the equations: Conservation of mass Equation of motion Conservation of energy Strain–displacement equations ∂(EPQ , θ , qrPQ ) RS = ρ0 ∂ERS ∂(EPQ , θ , qrPQ ) η=− ∂θ ε = ε(EPQ , θ , qrPQ ) or = (EPQ , θ , qrPQ ) hR = hR (EPQ , θ , θ,P , qrPQ ) r (E , θ , qr ) q˙ rRS = fRS PQ PQ

1 3 1 6 6

(8.33)

1 1 3 n

The 22 + n unknowns are ρ(1), RS (6), η(1), ε(1), hR (3), the displacements ui (3), ERS (6), θ (1), and qrRS (n), with the number of unknowns shown inside the parenthesis. Thus, the solution for the set of equations can be determined.

8.3.4

The Gibbs Formulation of Thermo-Mechanical Behavior

The Gibbs formulation is complementary to the Helmholtz formulation. In the Helmholtz formulation, strain is the independent variable and stress is the dependent variable; in the Gibbs formulation, stress is the independent variable and strain is the dependent variable. Thus, the state functions are functions of RS , θ , and qrRS . The energy equation is from (8.26) ε˙ =

1 ∂hR 1 RS E˙ RS − + q˙ ρ0 ρ0 ∂XR

(8.34)

For an irreversible system at constant qrRS , following Valanis [2], we may write ε˙ |qrPQ −

© 2005 by Chapman & Hall/CRC Press

1 RS E˙ RS = θ η| ˙ qrPQ ρ0

(8.35)

Internal Variable Theory and Endochronic Theory

409

Let = ε − ηθ , we have ˙ qr = ε˙ |qr − ηθ˙ − η| ˙ qrPQ θ | PQ PQ

(8.36)

Substituting (8.36) into (8.35), we obtain ˙ qr − | PQ

1 RS E˙ RS + ηθ˙ = 0 ρ0

(8.37)

The Gibbs free energy is now deﬁned as =−

1 RS ERS ρ0

(8.38)

By differentiation, we then have ˙ qr = | ˙ qr + | PQ PQ

1 1 ˙ RS ERS RS E˙ RS |qrPQ + ρ0 ρ0

(8.39)

Substituting (8.39) into (8.37), we obtain ∂ 1 ∂ ˙ RS + ˙ RS ERS + ηθ˙ = 0 θ˙ + ∂RS θ,qr ∂θ PQ ,qr ρ0 PQ

(8.40)

PQ

Since the stress and the temperature can be arbitrarily varied, it is concluded that ∂ ∂ (8.41) ERS = −ρ0 and η = − ∂RS θ,qr ∂θ PQ ,qr PQ

PQ

These are the constitutive equations in the Gibbs formulation. In the following functions, we note the differences in the independent variables: E = E(, θ, qr ), = (, θ, qr ), but = (E, θ , qr ). Differentiating (8.38), we have ˙ = ˙ −

1 1 ˙ RS ERS − RS E˙ RS ρ0 ρ0

(8.42)

or ∂ ∂ ∂ ˙ RS + θ˙ + r q˙ rRS ∂RS ∂θ ∂qRS =

∂ ˙ ∂ 1 1 ∂ ˙ RS ERS − RS E˙ RS ERS + θ˙ + r q˙ rRS − ∂ERS ∂θ ∂qRS ρ0 ρ0

© 2005 by Chapman & Hall/CRC Press

(8.43)

410

Continuum Mechanics and Plasticity

Using (8.14) and (8.41), (8.43) reduces to ∂ ∂ r q˙ RS = r q˙ rRS r ∂qRS ∂qRS

(8.44)

The Clausius–Duhem inequality (8.32) becomes ∂ r ∂ q˙ = r q˙ rRS ≤ 0 ∂qrRS RS ∂qRS

(8.45)

The evolution equations for qrRS are r (PQ , θ , qrPQ ) q˙ rRS = gRS

(8.46)

r must satisfy the constraint of Clausius–Duhem Note that the functions gRS r is related to f r by the inequality. In addition, from (8.31) and (8.46), gRS RS equation r r = fRS [EPQ (TU , θ , qsTU ), θ , qsTU ] gRS

with r, s = 1, . . . , n

(8.47)

r can be nonlinear. However, linear functions work extremely The functions gRS well for applications to be discussed in connection with the endochronic theory. In the case of linear functions, the evolution equations are

∂ + brRSPQ q˙ rPQ = 0 ∂qrRS

(r not summed)

(8.48)

where brRSPQ is a positive deﬁnite fourth-rank tensor. Knowing , an explicit form of constitutive equations can be obtained.

8.4 8.4.1

The Endochronic Theory of Plasticity The Concepts of the Endochronic Theory

Valanis developed the endochronic theory of plasticity in two major papers [6,7]. The Greek word endochronic means intrinsic (or internal) time. The deformation history is represented by a monotonically increasing time-like parameter ζ known as the endochronic (or intrinsic) time. The endochronic time accounts for the intrinsic material properties and is deﬁned as dζ 2 = PRSPQ dERS dEPQ

© 2005 by Chapman & Hall/CRC Press

(8.49)

Internal Variable Theory and Endochronic Theory

411

where PRSPQ is a fourth-rank tensor, which could depend on ERS . This concept of intrinsic time is different from that of Ilyushin [10] and Pipkin and Rivlin [11], using the arc length of the strain path as a parameter. In that case, dζ 2 = dERS dERS

(8.50)

We note that (8.50) is a special case of (8.49). Another original idea of Valanis’ is to develop a theory that describes the stress–strain curve without a yield surface. The stress–strain curves of metals such as aluminum, brass, and high-strength steel do not show an apparent yield point. As we have discussed in Section 6.2, several deﬁnitions of yield surfaces are available and there are factors affecting the experimental determination of yield surfaces. Valanis tried to avoid the use of yield surface and showed in [6] that, using the thermodynamics of the internal variable and the concept of intrinsic time, it was indeed possible to develop a theory which not only does not have a yield point but can also successfully describe metal behaviors such as the Baushinger effect in unloading behavior, hardening due to shear prestrain, cyclic stress–strain loops, and cyclic hardening. At the time when [6] was published, the ﬂow theory of plasticity was not yet successful in theoretically describing these complex behaviors of metals. This theory of Valanis [6] is simple in form and will be referred to as the simple endochronic theory. This theory has many advantages because of its simplicity in calculation. Take the cyclic loading as an example, the ﬂow theory of plasticity would need to determine whether the current state is in the plastic state and, if so, apply the ﬂow rule, which is incremental. An intense numerical integration is needed. The equations of the endochronic theory, on the other hand, may be integrated to obtain a closed form solution without having to determine the yield point. However, there are drawbacks of the simple endochronic theory. The unloading curve has a slope slightly larger than the initial slope of the stress–strain curve. If, in a plastic state, a small amount of stress unloading occurs and is immediately followed by a reloading back to the original stress level, then a stress–strain loop does not form. If this unloading–reloading cycle continues, then cyclic creep or ratcheting would occur without reaching a steady state, that is, the strain would continue to increase as the stress cycling continues, but not in agreement with experimental ﬁndings. Another drawback is related to the rate of entropy production. In a plastic state, increments in loading and unloading will result in the same rate of entropy production, which is not acceptable. Despite the drawbacks, the simple endochronic theory continues to be used by some investigators because of its simplicity and because the concept of yield surface is not needed. It provides a good approximation to metals when only loading is of interest, or under certain loading histories such as cyclic loading. An improved endochronic theory, or simply the “endochronic theory” in the remainder of this chapter, was proposed by Valanis [7] to remove the aforementioned drawbacks. The improved theory uses plastic strain to deﬁne the

© 2005 by Chapman & Hall/CRC Press

412

Continuum Mechanics and Plasticity

intrinsic time, while the simple endochronic theory uses the total strain. Valanis [7] showed that a limiting case of this new formulation leads to the deﬁnition of yield surface. In fact, the ﬂow theory of plasticity can be derived from the endochronic theory, including the ﬂow rule and the strainhardening rules. However, the forms of the ﬂow rule and strain-hardening rules are derived; whereas these forms and rules are separately assumed in the traditional ﬂow theory of plasticity. This author has been heavily involved in the development and veriﬁcation of the endochronic theory. Specially designed experiments have been conducted by the author and his coworkers which are then used to verify the theory. These investigations will be discussed in later sections of this chapter and in Chapter 9. 8.4.2

The Simple Endochronic Theory of Plasticity

The simple endochronic theory has been derived for small isothermal deformation in [6], using the Helmholtz formulation discussed in Section 8.3.3. In the small deformation, the stress is σ and the strain is ε. Equation (8.30) reduces to σ=

∂ , ∂ε

η=−

∂ , ∂θ

−

∂ · q˙ r ≥ 0 ∂qr

(r not summed)

(8.51)

From the last expression of (8.51), we see that q˙ r cannot be independent of −∂/∂qr . Otherwise, an arbitrary choice of q˙ r may violate the inequality. Therefore, q˙ r and −∂/∂qr must be related. The relation can be in the form of a function or of a functional, or something else. For the sake of simplicity, a function is assumed in the ensuing discussion. Furthermore, a linear form is assumed such that ∂ + brijkm q˙ rkm = 0 ∂qrij

(r not summed)

(8.52)

where brijkm is a symmetric positive deﬁnite tensor. Note that this linear form has been proven to be adequate in most applications. Other forms may be considered if called for. However, we like the linear form because of its mathematical simplicity. Substituting (8.52) into the last expression of (8.51), we obtain brijkm q˙ rij q˙ rkm ≥ 0

(r not summed)

(8.53)

The intrinsic time is from (8.49) dζ 2 = Pijkm dεij dεkm

© 2005 by Chapman & Hall/CRC Press

(8.54)

Internal Variable Theory and Endochronic Theory

413

In the endochronic theory, all developments are with respect to the increment of intrinsic time. The evolution equation for the internal variables can then be expressed with respect to the intrinsic time as dqr ∂ + brijkm (ζ ) km = 0 r ∂qij dζ

(r not summed)

(8.55)

where brijkm (ζ ) is a function of intrinsic time ζ and brijkm = (br0 )ijkm f (ζ ); (8.55) may then be written as dqr ∂ + (br0 )ijkm f (ζ ) km = 0 r ∂qij dζ

(r not summed)

(8.56)

or dqrkm ∂ r + (b ) =0 ijkm 0 ∂qrij dz

(r not summed)

(8.57)

where (br0 )ijkm is a fourth-rank constant tensor; the intrinsic time has been scaled by a factor f and z is the intrinsic timescale. The relation is dζ f (ζ )

dz =

(8.58)

The scaling factor f (ζ ) will be identiﬁed later as the isotropic hardening function. The case of f = 1 corresponds to no isotropic hardening. Generally, (8.58) may be integrated from the initial intrinsic time ζ0 to the current intrinsic time ζ as z=

ζ

ζ0

dζ f (ζ )

(8.59)

As a ﬁrst approximation, we use the linear form f (ζ ) = 1 + βζ

(8.60)

and, in this case, (8.59) becomes z=

1 ln(1 + βζ ) β

with initial values ζ0 = z0 = 0; β is a constant.

© 2005 by Chapman & Hall/CRC Press

(8.61)

414

Continuum Mechanics and Plasticity

In summary, the endochronic equations of the Helmholtz formulation for small isothermal deformation are = (ε, qr ), dz =

σ=

dζ , f (ζ )

∂ , ∂ε

r ∂ r dq + b = 0, · 0 ∂qr dz

(8.62)

dζ 2 = dε · P · dε

where a boldfaced letter with an underscore, such as P, denotes a fourth-rank tensor. To obtain an explicit constitutive equation, the free energy is expressed in a quadratic form as = 21 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr

(8.63)

where A , Br , Cr are fourth-rank constant tensors. Note that linear terms in ε are absent to accommodate the requirement that the reference state is unstressed. In addition, linear terms in qr are absent if the reversal of the sign of strain history leaves the form of the stress response invariant. Substituting (8.63) into (8.62), we obtain σ=A·ε+

Br · q r

Br · ε + Cr · qr + br0 ·

and

r

dqr =0 dz

(8.64)

If A, Br , Cr and br0 are isotropic functions and, since σ, ε, and qr are symmetric tensors, the isotropic expressions for these tensors are from (1.129) Aijkm = A1 δij δkm + A2 δik δjm ,

Brijkm = Br1 δij δkm + Br2 δik δjm ,

r Cijkm = C1r δij δkm + C2r δik δjm ,

(br0 )ijkm = br1 δij δkm + br2 δik δjm

(8.65)

Substituting (8.65) into (8.64) and separating the resulting equations into the hydrostatic and deviatoric parts, we ﬁnd σkk = (3A1 + A2 )εkk + (3Br1 + Br2 )qrkk σij

= A2 eij +

r

(8.66)

Br2 pijr

r

Br0 εkk + C0r qrkk + br0 Br2 eij + C2r pijr + br2

dqrkk =0 dz

dpijr dz

(r not summed)

(8.67)

=0

where the deviatoric parts are eij = εij − 13 δij εkk ,

© 2005 by Chapman & Hall/CRC Press

σij = σij − 13 δij σkk ,

pijr = qrij − 13 δij qrkk

(8.68)

Internal Variable Theory and Endochronic Theory

415

and A0 = 13 (3A1 + A2 ),

Br0 = 13 (3Br1 + Br2 ),

C0r = 13 (3C1r + C2r ),

br0 = 13 (3br1 + br2 )

(8.69)

Equations in (8.67) are constant coefﬁcient linear ordinary differential equations and the solutions are Br z Cr exp − r0 (z − z ) εkk (z ) dz with qrkk (0) = 0 qrkk = − r0 b0 z0 b0 (8.70) Br2 z C2r r

r exp − r (z − z ) eij (z ) dz with pij (0) = 0 pij = − r b2 z0 b2 Combining (8.66) and (8.70) yields σ =

1 σkk = 3

z z0

K(z − z )

dεkk dz dz

σij = 2

and

z

z0

µ(z − z )

deij dz dz (8.71)

where the kernel functions are given by K(z) = A0 −

(Br )2

2µ(z) = A2 −

0 C0r

r

(Br )2 2

r

C2r

H(z) +

(Br )2 0 C0r

r

H(z) +

e−λr z

(Br )2 2

r

C2r

with λr =

C0r br0 (8.72)

e−ρr z

Cr with ρr = r2 b2

where H(z) is the Heaviside step function. These kernel functions are also known as the heredity functions. If 2µ(z) is plotted against

z, the curve has a value of A2 at z = 0 and relaxes gradually to [A2 − r ((Br2 )2 /C2r )] as z increases and becomes large. Similarly, K(z) has an initial value of A0 and relaxes to

(A0 − r ((Br0 )2 /C0r )). The functions µ(z) and K(z) are sums of positive decaying exponential terms, where one or more of the exponents may be zero. This describes the effect of fading memory. In the event that the hydrostatic response is elastic as most metals are, Br0 = C0r = 0 and qrkk is constant. The ﬁrst equation of (8.72) reduces to K(z) = A0 H(z)

(8.73)

and the hydrostatic stress–strain curve is from (8.71) σ = 13 σkk = A0 εkk

© 2005 by Chapman & Hall/CRC Press

(8.74)

416

Continuum Mechanics and Plasticity

Valanis and Wu [12] investigated the representation of heredity functions and showed that the theory was able to describe observed behavior of metals under conditions of cyclic deformation. In addition, Wu and his coworkers [13–16] applied the theory to investigate the problem of viscoplastic wave propagation in thin rods and thin-walled tubes. By differentiation, the deviatoric part of the constitutive equation in (8.71) can be written in a differential form. In the simple case of µ(z) = µ0 e−αz , where µ0 and α are constants, we have σ = 2µ0

z

e−α(z−z )

0

de dz dz

(8.75)

and dσ = (−α)2µ0 dz

z

e−α(z−z )

0

de de dz + 2µ0

dz dz

(8.76)

or dσ de + ασ = 2µ0 dz dz

(8.77)

This is the constitutive equation in the differential form. From (8.77), we see that the plastic strain increment is dep = de −

dσ α = dzσ 2µ0 2µ0

(8.78)

This is in the form of the Prandtl–Reuss relation, when the elastic strain is considered. On the other hand, the function µ(z) may contain more terms. For example, µ(z) = µ0 + µ1 e−αz , where µ0 , µ1 , and α are constants. We then obtain dep =

α µ0 σ dz − αe dz 2µ¯ µ¯

with µ¯ = µ0 + µ1

(8.79)

Equation (8.79) is not in the form of the Prandtl–Reuss relation. EXAMPLE 8.1

Determine the endochronic constitutive equation for uniaxial

tension. Solution In uniaxial tension, (8.71) reduces to σ =

© 2005 by Chapman & Hall/CRC Press

z 0

E(z − z )

dε dz dz

(a)

Internal Variable Theory and Endochronic Theory

417

The stress is σ , the strain is ε, and E(z) is the heredity function. We assume that the specimen is initially in an annealed state so that z0 = 0. We consider the simplest case possible, when E(z) has only one exponential term, that is, E(z) = E0 e−αz

(b)

where E0 and α are constants. The intrinsic time increment is from (8.54) dζ = ±k dε

(c)

in which k is assumed to be a constant for simplicity. The positive and negative sign in (c) are for loading and unloading. We use the linear form for intrinsic timescale given by (8.60), which is integrated to yield (8.61). We then obtain from (8.61) the expression 1 + βζ = eβz , which leads to dζ = eβz dz

(d)

where β is a constant. Substituting (b) into (a) and using (c) and (d), we obtain σ = E0

z

e−α(z−z )

0

dε dζ dz = E0 dζ dz

z

e−α(z−z )

0

1

(eβz )dz k

eβz

E0 E0 (1 + βζ ) [1 − e−(α+β)z ] = [1 − (1 + βζ )−(1+α/β) ] k(α + β) kβ(1 + α/β) α E0 1 with n = 1 + = (1 + βζ ) 1 − kβn (1 + βζ )n β

=

(e)

In loading starting from zero load and zero strain, (c) can be integrated to yield ζ = kε

(f)

Using (f), (e) becomes σ =

E0 1 (1 + β1 ε) 1 − β1 n (1 + β1 ε)n

with β1 = kβ

(g)

This is the endochronic stress–strain relation with three parameters E0 , β1 , and n. This equation is able to describe the stress–strain curve for most metallic materials. The three parameters may be determined by a method described in Example 8.2. A method by use of the optimization technique is given by Jao et al. [17].

© 2005 by Chapman & Hall/CRC Press

418

Continuum Mechanics and Plasticity Et

0

E0 FIGURE 8.3 A stress–strain curve.

EXAMPLE 8.2

Determine the three parameters of the endochronic stress–

strain relation σ =

E0 1 (1 + β1 ε) 1 − β1 n (1 + β1 ε)n

(a)

Solution A hypothetical experimental stress–strain curve is shown in Figure 8.3, and we like to determine E0 , β1 , and n so that (a) describes this experimental curve. We ﬁrst determine E0 , Et , and σ 0 from the experimental curve. E0 is the slope at ε = 0; Et is the tangent modulus at large ε; and σ 0 is the intercept of the asymptote of the stress–strain curve with the stress axis. We note that E0 = (dσ /dε)|ε→0 , and this is about the same as Young’s modulus for materials that has a very straight initial curve. E0 should be slightly larger than the conventional value for Young’s modulus, if the material starts to bend right from the beginning of the stress–strain curve. The asymptote at large ε is found from (a) as σ =

E0 (1 + β1 ε) β1 n

(b)

with slope dσ E0 Et = = dε ε→large n

(c)

Therefore, n=

© 2005 by Chapman & Hall/CRC Press

E0 Et

(d)

Internal Variable Theory and Endochronic Theory

419

The intercept of the asymptote with the stress axis is found by setting ε = 0 in (b). Thus, σ0 =

E0 β1 n

(e)

β1 =

E0 nσ 0

(f)

From (e), we obtain

Therefore, knowing E0 , Et , and σ 0 , we ﬁnd n from (d) and β1 from (f). EXAMPLE 8.3

If the free energy is positive deﬁnite, that is, = 12 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr > 0

(a)

and if r Cijkm = C1r δij δkm + C2r δik δjm

Aijkm = A1 δij δkm + A2 δik δjm ,

(b)

show that A1 + 13 A2 > 0,

A2 > 0

and

C1r + 13 C2r > 0,

C2r > 0

(c)

Solution The free energy is positive deﬁnite, > 0, for any ε and qr subjected to the thermodynamic constraints discussed in Section 8.3.3. In a special case, > 0 for ε = 0 and arbitrary nonzero qr , so that = 12 qr · Cr · qr > 0

(d)

Therefore, Cr must be positive deﬁnite. Another special case is when qr = 0 subjected to nonzero arbitrary ε. Then, = 12 ε · A · ε > 0

(e)

that is, A must be positive deﬁnite. Using (b) and (e), we have = 12 (A1 εii εkk + A2 εik εik )

© 2005 by Chapman & Hall/CRC Press

(f)

420

Continuum Mechanics and Plasticity

which may be written in the matrix form as T ε11 ε22 ε33 ε12 1 T ε13 = [ε] [A][ε] = 2 ε 21 ε21 ε31 ε32 A1 A1 0 0 0 0 0 0 ε11 A1 + A2 ε22 A1 A + A A 0 0 0 0 0 0 1 2 1 A1 A1 A1 + A 2 0 0 0 0 0 0 ε33 0 0 0 2A2 0 0 0 0 0 ε12 0 0 0 0 2A2 0 0 0 0 ε13 × 0 0 0 0 0 0 0 2A2 0 ε21 0 0 0 0 0 0 2A2 0 0 ε21 0 0 0 0 0 0 0 2A2 0 ε31 ε32 0 0 0 0 0 0 0 0 2A2 (g)

Since is positive deﬁnite, [A] is a positive deﬁnite matrix, that is, the determinant of every principal minor should be nonnegative. Therefore, (a) A1 + A2 > 0

(h)

A1 + A2 (b) A1

= A2 (2A1 + A2 ) > 0 A1 + A 2

A1 + A2 (c) A1 A1

A1 A1 + A 2 A1

A1 A1 = A22 (3A1 + A2 ) > 0 A1 + A 2

A1 A1 + A 2 A1 0

A1 A1 A1 + A 2 0

A1 + A2 A1 (d) A1 0

A1

(i)

0 0 = (2A2 )A2 (3A1 + A2 ) > 0 2 0 2A2

(j)

(k)

From (h) to (k), it is concluded that A2 > 0,

A1 + A2 > 0,

© 2005 by Chapman & Hall/CRC Press

2A1 + A2 > 0,

3A1 + A2 > 0

(m)

Internal Variable Theory and Endochronic Theory

421

Plotting the above inequalities in the A2 versus A1 space, it is found that the solution is bounded by A2 > 0

3A1 + A2 > 0

and

(n)

Using a similar procedure, the following inequalities can be established C1r + 13 C2r > 0

and

C2r > 0

(o)

An alternate proof is obtained by considering simple loading conditions. We rewrite (f) as A2 1 1 (p) A1 + (εkk )2 + A2 eik eik = 2 3 2 In the case of hydrostatic strain, the strain components are ε11 = ε22 = ε33 = ε and eij = 0, (p) reduces to =

1 A2 A1 + (3ε)2 > 0 2 3

or

A1 +

A2 >0 3

(q)

In the case of shear with ε12 = 0 and other εij = 0, we have from (p) = A2 (e12 )2 > 0

or

A2 > 0

(r)

The physical meanings are not clear if the same procedure is applied to = 12 qr · Cr · qr > 0. 8.4.3

The Improved Endochronic Theory of Plasticity

Valanis [7] used a strain-like tensor Qij to deﬁne the intrinsic time as dζ 2 = dQij dQij

where Qij = εij − Kijkm σkm

(8.80)

This deﬁnition of intrinsic time is a generalization of (8.54). In onedimensional straining, (8.80) reduces to dσ dζ = |Q| = dε − k1 E 0

with 0 ≤ k1 ≤ 1

(8.81)

When k1 = 0, dζ = |dε|, which is the simple endochronic theory; but when k1 = 1, Q has the meaning of plastic strain. This new deﬁnition of intrinsic time removes the drawbacks mentioned for the simple endochronic theory, and, in addition, the case of k1 = 1 leads to the existence of yield surface. We shall demonstrate the latter assertion in the discussions to follow.

© 2005 by Chapman & Hall/CRC Press

422

Continuum Mechanics and Plasticity

We ﬁrst show that the deviatoric constitutive equation of (8.71) σ = 2

z

z0

µ(z − z )

de dz = 2µ0 dz

z z0

ξ(z − z )

de dz dz

(8.82)

may be written in the following form σ = 2µ0

z 0

ρ(z − z )

dQ dz dz

(8.83)

where Q = e − k1

σ , 2µ0

µ(z) = µ0 ξ(z),

ξ(0) = 1

(8.84)

The relation between ξ(z) and ρ(z) may be found by the method of Laplace transformation. From (8.82), we have σ¯ = 2µ0 ξ¯ p¯e

with e(0) = 0

(8.85)

where f¯(p) is the transform of the function f (z) and p is the parameter of Laplace transformation. We note that L(df (z)/dz) = pf¯(p) − f (0). On the other hand, (8.83) is transformed into ¯ ¯ Q σ¯ = 2µ0 ρp

with Q(0) = 0

(8.86)

Using the Laplace transform of (8.84), (8.86) is further written as

σ¯ = 2µ0 ρp ¯ e¯ − k1

σ¯ 2µ0

(8.87)

Substituting (8.85) into (8.87), the resulting equation is ¯ ξ¯ = ξ¯ ρ¯ − k1 ρp

(8.88)

¯ ξ¯ − ξ(0)) − k1 ρξ(0) ¯ = ξ¯ ρ¯ − k1 ρ(p

(8.89)

which may be written as

An inverse transform of (8.89) gives us (1 − k1 )ρ(z) − k1

© 2005 by Chapman & Hall/CRC Press

z 0

ρ(z − z )

dξ dz = ξ(z) dz

with ξ(0) = 1

(8.90)

Internal Variable Theory and Endochronic Theory

423

It can be shown that, for k1 = 1, the solution of (8.90) is ρ(z) = ρ0 δ(z) + ρ1 (z)

(8.91)

where ρ1 (z) =

n−1

Rr e−βr z ,

ξ(z) =

r=1

n

ξr e−αr z ,

r=1

n

ξr = 1

(8.92)

r=1

and δ(z) is the Dirac delta function; Rr , ξr , βr , αr , and ρ0 are constants. Using (8.91) and (8.92), (8.83) becomes σ = 2µ0 ρ0

dQ(z) + 2µ0 dz

z 0

ρ1 (z − z )

dQ(z ) dz dz

(8.93)

Equation (8.93) is the constitutive equation of the endochronic theory. This equation may be used directly to calculate the stress–strain response curves. On the other hand, based on this equation, the ﬂow rule, the yield surface, and its hardening rules can be derived, thereby establishing a connection between the present theory and the ﬂow theory of plasticity. By doing so, the physical meanings of some functions and parameters of this theory become clear. The differences between this theory and the ﬂow theory are that the forms of the ﬂow rule, yield surface, and hardening rule are related in this theory and they evolve with respect to the intrinsic time, while they are quite open to differently proposed forms in the classical ﬂow theory. In the following subsection, we derive the ﬂow rule, the yield surface, and the hardening rule. EXAMPLE 8.4

In the simple case of ξ(z) = ξ1 e−α1 z + ξ2 e−α2 z

(a)

determine the expression for ρ(z). Solution The Laplace transform of (a) is ξ¯ (p) =

ξ1 ξ2 + p + α1 p + α2

(b)

Substituting (b) into (8.88), we have ρ¯ =

ξ¯ (p) p+λ = 2 ¯ (1 − k1 )p + (α1 + α2 − k1 λ)p + α1 α2 1 − k1 pξ (p)

© 2005 by Chapman & Hall/CRC Press

(c)

424

Continuum Mechanics and Plasticity

where λ = ξ1 α2 + ξ2 α1 . In the case of k1 → 1, (c) becomes ρ¯ ≈

p+λ p+λ = (1 − k1 )(p + β1 )(p + β2 ) (1 − k1 )p2 + (α1 + α2 − λ)p + α1 α2

(d)

where β1 =

λ¯ , 1 − k1

β2 =

α1 α2 , λ¯

λ¯ = α1 ξ1 + α2 ξ2

(e)

Equation (d) may be further written as ρ¯ =

1 1 − k1

((λ − β1 )/(β2 − β2 )) ((λ − β2 )/(β1 − β2 )) + p + β1 p + β2

(f)

which may then be inverse transformed into 1 ρ(z) = 1 − k1

λ − β1 −β1 z λ − β2 −β2 z e + e β2 − β 1 β1 − β 2

(g)

Using (e), we ﬁnd that λ − β1 ≈1 β2 − β 1

and

λ − β2 1 λλ¯ − α1 α2 ≈ 1 − k 1 β1 − β 2 λ¯ 2

(h)

Therefore, (g) becomes 1 α1 α2 λ¯ λλ¯ − α1 α2 ρ(z) = exp − exp − z + z 1 − k1 1 − k1 λ¯ 2 λ¯

(i)

When k1 → 1, (i) reduces to ρ(z) = ρ0 δ(z) +

λλ¯ − α1 α2 λ¯ 2

α1 α2 exp − z = ρ0 δ(z) + ρ1 (z) λ¯

(j)

Thus, ρ1 (z) =

© 2005 by Chapman & Hall/CRC Press

λλ¯ − α1 α2 λ¯ 2

α1 α2 exp − z λ¯

(k)

Internal Variable Theory and Endochronic Theory 8.4.4

425

Derivation of the Flow Theory of Plasticity from Endochronic Theory

In the case of k1 = 1, the deviatoric part of the endochronic constitutive equation is from (8.93) σ = 2µ0 ρ0

dQ(z) + 2µ0 dz

z 0

ρ1 (z − z )

dQ(z ) dz dz

(8.93)

with the intrinsic time deﬁned from (8.80) by p

dζ 2 = dQij dQij

where dQij = dεij = deij −

dσij 2µ0

(8.94)

If we let α = 2µ0

z 0

ρ1 (z − z )

dQ(z ) dz dz

and

σy = 2µ0 ρ0

(8.95)

then, (8.93) can be written as dQ f (z) + α dζ

(8.96)

dζ (σ − α) σy f (z)

(8.97)

σ = σy which may be further written as dQ =

This equation may be considered as the ﬂow rule using the concept of the ﬂow theory of plasticity. By substituting (8.97) into (8.94), we obtain 2

dζ = dQ · dQ =

dζ

σy f (z)

2 (σ − α) · (σ − α)

(8.98)

or [(σ − α) · (σ − α) − (σy f (z))2 ]dζ 2 = 0

(8.99)

Therefore, we obtain from (8.99) either (σ − α) · (σ − α) = (σy f (z))2

with dζ 2 = 0

(8.100)

or dζ 2 = 0

© 2005 by Chapman & Hall/CRC Press

(8.101)

426

Continuum Mechanics and Plasticity

Equation (8.100) is the yield criterion with combined isotropic–kinematic hardening. α represents the back stress and f (z) represents the isotropic hardening. We will call f (z) the isotropic-hardening function. The yield criterion applies when p

p

dζ 2 = dQij dQij = dεij dεij p

p

p

p

p

p

= (dε11 )2 + (dε22 )2 + (dε33 )2 + 2(dε12 )2 + 2(dε23 )2 + 2(dε31 )2 = 0 (8.102) p

Since all terms in (8.102) are positive, dεij = 0 when dζ 2 = 0. dζ 2 = 0 only when all components of the plastic strain increments are zero. The case of dζ 2 = 0 is given by (8.101) and further written as 2

dζ =

p p dεij dεij

= deij −

dσij

dσij

deij − 2µ0 2µ0 dσ 2 dσ 2 dσ 2 = de11 − 11 + de22 − 22 + de33 − 33 2µ0 2µ0 2µ0 2 2

2 dσ12 dσ23 dσ31 + 2 de12 − + 2 de23 − + 2 de31 − =0 2µ0 2µ0 2µ0 (8.103)

Since all terms in (8.103) are positive, dζ 2 = 0 only when all terms are zero, that is, deij −

dσij 2µ0

=0

or

dσij = 2µ0 deij

and

σij = 2µ0 eij

(8.104)

When all components of the plastic strain increments are zero, the material behavior is described by (8.104), which is the elastic constitutive equation. We have thus shown that the ﬂow theory of plasticity may be derived from the endochronic theory when k1 = 1. The yield function is given by (8.100); the ﬂow rule is given by (8.97); the back stress is given by (8.95); and the isotropic hardening is given by the function f (z). We see from (8.97) that the normality condition between the plastic strain increment and the yield surface (8.100) is satisﬁed. The evolution of back stress may be written in a differential form by differentiating (8.95). If, for simplicity, only one exponential term is used in ρ1 (z), that is, ρ1 (z) = ρˆ e−αz , where ρˆ and α are constants, then α = 2µ0 ρˆ

© 2005 by Chapman & Hall/CRC Press

0

z

e−α(z−z )

dεp (z ) dz dz

(8.105)

Internal Variable Theory and Endochronic Theory

427

and dα dεp = 2µ0 ρˆ − αα dz dz

(8.106)

This is a nonlinear evolution equation for α and was used by Wu and Yang [18] and Wu et al. [19] as mentioned in Section 6.5.3. This equation is also known as the Armstrong–Frederick evolution equation. Another special case of (8.95) is when ρ1 (z) = ρˆ = constant. In this case, (8.95) becomes α = 2µ0 ρε ˆ p

or

dα = c dεp

with c = 2µ0 ρˆ

(8.107)

which is the linear kinematic hardening of Prager [20] and Ziegler [21]. In the general case, when ρ1 (z) is given by (8.92), the evolution equation for α is dεp dα 2G0 Rr β r αr = − dz dz n−1

n−1

r=1

8.4.5

with α =

r=1

n−1

αr

(8.108)

r=1

Applications of the Endochronic Theory to Metals

The endochronic theory is applied to describe several aspects of metallic deformation. They include loading–unloading, cyclic loading, loading with multi-axial strain paths, and the viscoplastic effect. Additional applications will be discussed in Chapter 9. 8.4.5.1

The loading–unloading stress–strain curves

In the case of uniaxial stress, the endochronic constitutive equation is σ = E0

z 0

ρ(z − z )

dε p dz dz

(8.109)

We investigate three functional forms of the isotropic-hardening function f (z). They are: Form (a): f (z) = eβz , and

Form (b): f (z) = C − (C − 1)e−βc z ,

Form (c): f (z) = e−βs z

(8.110)

The equation dζ /dz = f (z) is plotted in the ζ versus z space in Figure 8.4(a) for the three forms. The slope of the asymptote for form (a) is ∞, that for form (b) is C, and for form (c) is 0. The curve of form (c) approaches a value of 1/βs when z is large. The straight line at 45◦ angle is the case of f (z) = 1, which represents the nonhardening behavior. This line separates the ζ –z space into hardening zone and softening zone. When form (b) is used, the value of C dictates the material behavior. The case of C > 1 corresponds to strain

© 2005 by Chapman & Hall/CRC Press

428

Continuum Mechanics and Plasticity

(a) 10

(b)

C>1

10

8

f = C–(C–1)e–z, final slope = C

6 4

2

6 0C z∗ and the integral in (8.109) is divided into two integrals σ = E0

z∗ 0

ρ(z − z )

dε p dz + E0 dz

z z∗

ρ(z − z )

dε p dz dz

(8.116)

Using (8.111) as the kernel function, the ﬁrst integral of (8.116) consists of three terms. They are E0

0

E1

z∗

z∗

0

δ(z − z )[C − (C − 1)e−βc z ]dz = 0,

= E1 e E2

z∗

0

e−α(z−z ) [C − (C − 1)e−βc z ]dz −αz

C −αz∗ C − 1 −(βc −α)z∗ − 1) + − 1) , (e (e α βc − α

(8.117)

dζ dz = E2 ζ ∗ dz

The second integral also has three terms, given by

z

z∗ z

E0 E1

z∗

δ(z − z )(−1)[C − (C − 1)e−βc z ]dz = −σy [C − (C − 1)e−βc z ],

= −E1 E2

z 0

e−α(z−z ) (−1)[C − (C − 1)e−βc z ]dz

(−1)

C C − 1 −βc z ∗ ∗ ∗ (e − e−α(z−z )−βc z ) (1 − e−α(z−z ) ) + α α − βc

(8.118)

dζ dz = −E2 (ζ − ζ ∗ ) dz

Using (8.117) and (8.118), (8.116) is reduced to σ = − σy [C − (C − 1)e −

−βc z

]+

σ0 ∗ − σy C[2 e−α(z−z ) − e−αz − 1] C

σ0 C−1 ∗ ∗ [2 e−α(z−z )−βc z − e−αz − e−βc z ] + E2 (2ζ ∗ − ζ ) − σy α C α − βc (8.119)

During the unloading stage, the following relation holds dζ = −dεp

© 2005 by Chapman & Hall/CRC Press

∗

with initial condition ζ ∗ = εp

(8.120)

Internal Variable Theory and Endochronic Theory

431

Integration of (8.120) results in ε p = 2ζ ∗ − ζ

(8.121)

The loading–unloading curves have been calculated and compared with experimental results for 304 stainless steel by Wu and Yip [22]. 8.4.5.2

A strain-controlled cyclic loading

Since most experiments have been conducted by controlling the total strain amplitude ε, a small amount of approximation is involved in this theoretical representation by considering a constant plastic strain amplitude cycling. Figure 8.6(a) shows a schematic drawing for strain cycles plotted against time t and the notation used to denote intrinsic time z at each half cycle. Figure 8.6(b) shows the corresponding cyclic stress–strain curve. The loading in the previous subsection can be viewed as the ﬁrst 41 cycle which is valid (a) Strain Control

z3*

z*

z7*

z5*

t

z2*

z4*

∆

z6*

(b) Cyclic Hardening Hysteresis Loops z(2N)* z5* z3* z* Stable

1 D

D

z2* z4* z(2N)* FIGURE 8.6 (a) Strain cycles against time, (b) cyclic hardening hysteresis loops (From Wu, H.C. and Yip, M.C., J. Eng. Mater. Technol., 103, 212, 1981. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

432

Continuum Mechanics and Plasticity

for 0 < z < z∗ and the unloading in the previous subsection can be viewed as the ﬁrst unloading of the cyclic loading valid for z∗ < z < z∗∗ . We continue to derive the equations for the ﬁrst reloading and the subsequent loading. ∗ Using the same procedure, the ﬁrst reloading is valid for z∗∗ < z < z3 and the equation has been found to be σ0 ∗∗ σ = σy [C − (C − 1)e ]+ − σy C[−2 e−α(z−z ) C C−1 σ0 −α(z−z∗ ) −α + 2e − e z + 1] − − σy α C α − βc −βc z

× [−2e−α(z−z

∗∗ )−β z∗∗ c

+ 2e−α(z−z

+ E2 (ζ + 2ζ ∗ − 2ζ ∗∗ )

∗ )−β z∗ c

− e−αz + e−βc z ]

with ε p = 2ζ ∗ − 2ζ ∗∗ + ζ

(8.122)

This procedure may be continued. A general expression of the response function for the constant total strain amplitude cyclic loading test may be found to be σ = (−1)2N σy [C − (C − 1)e−βc z ] σ0 ∗ ∗∗ − σy C{1 − e−αz + 2[e−α(z−z ) − 1] − 2[e−α(z−z ) − 1] + C 2N ∗

+ · · · − [(−1)2N 2][e−α(z−z ) − 1]} σ0 α(C − 1) −βc z ∗ ∗ − {e − e−αz + 2[e−α(z−z )−βc z − e−βc z ] − σy C α − βc − · · · − (−1)2N 2[e−α(z−z + E2 ε p

for z > z2N

2N ∗ )−β z2N ∗ c

− e−βc z ]}

∗

(8.123)

where ∗

εp = ζ + 2(ζ ∗ − ζ ) − 2(ζ ∗∗ − ζ ) + · · · − (−1)2N · 2(ζ 2N − ζ )

(8.124) ∗

and N = 12 , 1, 1 12 , 2, . . . . If the above equation is examined at z = z2N ∗ and z = z2N + , a ∗drop or jump in stress of magnitude 2σy f (z) = 2N 2σy [C − (C − 1)e−βc z ] results, which corresponds to the elastic response upon reversal of loading direction. The magnitude of the jump in stress is determined by the isotropic expansion of the yield surface. For a sufﬁciently large z, the hysteresis loop becomes steady. In this case the jump or drop in stress becomes a constant value of 2Cσy .

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

433

MPa ksi Cyclic Stress–strain Curve

12½ Stable

150 20

3½

100

2½ 10

50

1½ N=½

–1.0

–0.6

–0.2

0.2

0.6

1.0

%

–50 –10 –100 –150

Theory

–20 Experiment from [23] N = ½ and 1 N = 1½ and 2 N = 2½ and 3 N = 3½ and 4 N = 8½ and 9 (Stable)

FIGURE 8.7 Theory and experimental data (From Wu, H.C. and Yip, M.C., J. Eng. Mater. Technol., 103, 212, 1981. With permission from ASME).

We now use (8.123) to predict the cyclic stress–strain loops experimentally obtained by Lamba and Sidebottom [23]. These authors obtained cyclic stress– strain curves of oxygen-free high-conductivity copper covering curves from the ﬁrst cycle to the stable loop. The hardening effect was extremely rapid in the ﬁrst few cycles of the test. After further reversals, hardening ceased and a steady stress range was achieved. Figure 8.7 illustrates the experimental data and the theoretical prediction from (8.123). The material parameters used in the calculation are: σ 0 = 25 ksi (1.73 × 102 MPa), σy = 2 ksi (13.78 MPa), E2 = 0, C = 8.75, βc = 40, α = 3000, and ε = 1.75%. Finally, we mention that the same theory was applied by Wu et al. [24] to investigate the problem of cyclic full-reversed torsional loading of a solid bar with circular cross-section. Numerical techniques were employed to obtain the solution. The parameters of the constitutive model were determined from the test data of thin-walled specimens. These parameters were then used without alteration to compute stress distributions within the solid specimen.

© 2005 by Chapman & Hall/CRC Press

434

Continuum Mechanics and Plasticity

Special attention was given to the residual stress distribution. Reasonable results were obtained. The relation of torque versus strain at the outermost ﬁber of the solid specimen provided an ultimate check of the theory as applied to this case.

8.4.5.3 Loading with multiaxial strain path From (8.93), the constitutive equation for metals is

σ =

dε σy

p (z)

dz

+ 2µ2

z

e−α(z−z )

0

dε p (z ) dz + 2µ1 ε p dz

(8.125)

where σy is the deviatoric yield stress; µ1 and µ2 are constants. The volumetric behavior is elastic, given by (8.74). Only one exponential term in the kernel function is used for simplicity. We applied (8.125) to describe two strain-controlled combined axial–torsion tests (paths 01A and 02B) shown in Figure 8.8. Form (b) of (8.110) is the isotropic-hardening function used in this derivation. The state of stress and its deviator and the plastic strain are 2σ 3

[σ ] = τ 0

σ τ 0 [σ ] = τ 0 0 , 0 0 0

τ σ − 3 0

p ηp 0 ε p εp η − p 0 [ε ] = 2 εp 0 0 − 2 (8.126)

0

0 , σ − 3

where ηp is the tensorial shear strain. The intrinsic time is obtained from dζ 2 = dε p · K · dε p

B

1

0 FIGURE 8.8 Two strain paths of combined axial–torsion.

© 2005 by Chapman & Hall/CRC Press

(8.127)

A

2

Internal Variable Theory and Endochronic Theory

435

as dζ = [k12 (dε p )2 + k22 (dηp )2 ]1/2

(8.128)

where k1 and k2 are constants. We follow the work of Wu and Yang [25] in the following discussion with permission from Elsevier. (A) Path 01A The specimen is ﬁrst strained in pure torsion from 0 to 1 (Figure 8.8) and then strained in tension from 1 to A while keeping the total shear strain constant. p The plastic shear strain at 1 is denoted by η∗ , the corresponding shear stress ∗ ∗ by τ , and the intrinsic time by z . There are two stages in this path. The ﬁrst stage is straining from 0 to 1 and the second stage from 1 to A. We have a pure torsion in the ﬁrst stage and the equations are from (8.125) τ=

dη σy

p

+ 2µ2

dz

z

e−α(z−z )

0

dηp dz + 2µ1 ηp dz

and

σ =0

(8.129)

Since during this stage, dζ = k2 dηp , (8.129) may be integrated. In the second stage, (8.125) gives σ = 1.5

dε σy

p

dz

+ 2µ2

z z∗

e

−α(z−z ) dε

p

dz

dz + 2µ1 ε

p

(8.130)

and τ = σy

dηp + 2µ2 X e−αz + 2µ2 dz

z z∗

e−α(z−z )

dηp dz + 2µ1 ηp dz

(8.131)

where X=

0

z∗

eαz

dηp 1 dz =

dz k2

C αz∗ C − 1 (α−β)z∗ − 1] [e − 1] − [e α α−β

(8.132)

Equation (8.131) may be reduced to a closed-form expression for τ in terms of z, which is accomplished by use of the following procedure. We note that η remains constant during this stage and we have dηp = −

dτ 2µ0

(8.133)

in which µ0 is the shear modulus. (8.133) is then integrated to yield p

ηp = η∗ −

© 2005 by Chapman & Hall/CRC Press

1 (τ − τ ∗ ) 2µ0

(8.134)

436

Continuum Mechanics and Plasticity

Letting z −z∗ = t and z −z∗ = t and making use of (8.133) and (8.134), (8.131) may be written as −σy dτ µ2 t −α(t−t ) dτ −α(t+z∗ ) τ= + 2µ2 e X− e dt 2µ0 dt µ0 0 dt 1 p + 2µ1 η∗ − (t − t∗ ) 2µ0

(8.135)

Laplace transform of (8.135) gives τ¯ =

¯ Q R¯ ∗

=

p

p{(p + α)σy τ ∗ + 4µ0 µ2 e−αz X + 2µ2 τ ∗ } + 4µ0 µ1 (η∗ + (τ ∗ /2µ0 ))(p + α) p{σy p2 + [ασy + 2(µ0 + µ1 + µ2 )]p + 2(µ0 + µ1 )α} (8.136)

which, by partial fraction, can be reduced to τ¯ =

2 µ 0 µ1 p µ0 + µ 1

p

η∗ +

τ∗ 2µ0

+

A B +

p−α p − β

(8.137)

where τ¯ is the Laplace transform of τ (z) and A, B, α , β are constants. Con¯ ¯ )/R¯ (α ), B = Q(β ¯ )/R¯ (β ), = 0; A = Q(α stants α and β are the zeros of R(p)

¯ ¯ ¯ and R¯ (p) = dR/dp. The functions Q(p) and R(p) are deﬁned in (8.136). Finally, (8.137) may be inverted to yield τ=

2µ0 µ1 µ0 + µ 1

p

η∗ +

τ∗ 2µ0

∗

+ A eα (z−z ) + B eβ (z−z

∗)

(8.138)

which is the expression relating τ to z. The equation for axial stress (8.130) may be written in a form convenient z

for numerical computation. Let S = z∗ e−α(z−z ) (dε p /dz )dz ; then by differentiating this integral with respect to z, we obtain dS dεp = − αS dz dz

(8.139)

in which, when dε p /dz is known, S may be computed step by step. Thus, σ may be found from dε p σ = 1.5 σy + 2µ2 S + 3µ1 ε p dz

© 2005 by Chapman & Hall/CRC Press

(8.140)

Internal Variable Theory and Endochronic Theory

437

The quantity dε p /dz is computed from the equation below which is found from (8.128) and (8.133)

dε p dz

2

1

=

k12

dζ dz

2

−

k2 2G0

2

dτ dz

2 (8.141)

The quantity dζ /dz is given by form (b) of (8.110) and dτ/dz is found by differentiation of (8.138). Therefore, by assuming a value for z, τ , and dτ/dz may be computed from (8.138), and dεp /dz may be found from (8.141). Using the latter value, S can be found step by step from (8.139) and σ can be obtained from (8.140). Furthermore, knowing the value of dε p /dz and using (8.133), ε p and ηp can be computed. (B) Path 02B The specimen is ﬁrst strained in pure tension from 0 to 2 (Figure 8.8) and then strained in torsion from 2 to B while keeping the total axial strain constant. p The plastic tensile strain at 2 is denoted by ε∗ , the corresponding tensile stress ∗ ∗ by σ , and the intrinsic time by zˆ . There are two stages in this path. The ﬁrst stage is straining in pure tension from 0 to 2, and the second stage from 2 to B. The equations for stage 1 are

dε σy

σ = 1.5

p

dz

+ 2µ2

z

e

−α(z−z ) dε

p

dz

0

dz + 2µ1 ε

p

τ =0

and

(8.142) and the equations for stage 2 are z p dε p

dε e−α(z−z ) dz + 2µ1 ε p + 2µ2 Y e−αz + 2µ2 σ = 1.5 σy dz dz zˆ ∗

(8.143)

and τ=

dη σy

p

dz

+ 2µ2

z zˆ ∗

e−α(z−z )

dηp dz + 2µ1 ηp dz

(8.144)

where Y=

zˆ ∗

e 0

αz dε

p

1 dz = dz k1

C αˆz∗ C − 1 (α−β)ˆz∗ [e − 1] − [e − 1] α α−β

(8.145)

Following a similar procedure as in Path 01A, we ﬁnd E0 Et σ = E0 + E t

© 2005 by Chapman & Hall/CRC Press

p ε∗

σ∗ + E0

ˆ eαˆ (z−ˆz∗ ) + Bˆ eβˆ (z−ˆz∗ ) +A

(8.146)

438

Continuum Mechanics and Plasticity

dε p = − Sˆ =

z

zˆ ∗

dσ E0

e−α(z−z )

(8.147)

dηp dz dz

(8.148)

dηp dSˆ = − α Sˆ dz dz dηp + 2µ2 Sˆ + 2µ1 ηp τ = σy dz

(8.149) (8.150)

and

dηp dz

2

=

1 k22

dζ dz

2

−

k1 E0

2

dσ dz

2 (8.151)

ˆ Bˆ are constants; E0 is Young’s modulus and Et = 3µ1 . in which αˆ , βˆ , A, Assuming a value for z, σ , and dσ/dz may be computed from (8.146), and dηp /dz may be found from (8.151). Using the latter value, Sˆ can be found step by step from (8.149) and τ can be obtained from (8.150). Furthermore, knowing the value of dηp /dz and using (8.147), ε p and ηp can be computed. For the purpose of assessing the validity of the derived equations, the theoretical results are compared with the experimental data obtained by Ohashi et al. [26] for thin-walled tubular brass (60% Cu, 40% Zn) specimens. The constants of the theory have been determined in [25] to be σy = 95.02 MPa, β = 4.3996, C = 4.5799, µ0 = 12.74 GPa, µ2 = 6.37 GPa, µ1 = 49.0 MPa, k1 = 1, and α = 500. The material response for Path 01A is shown in Figure 8.9 after torsion prestrain of ηp = 4.33 × 10−3 , 8.66 × 10−3 , 17.32 × 10−3 , and 25.98 × 10−3 . It is seen that the theory agrees well qualitatively with the experiment. There are quantitative discrepancies between the theory and experiment at the knee portion of the axial stress curve, however. In addition, the theory predicted a faster relaxation of shear stress than the experimental data indicated. Ohashi and his coworkers [27,28] have described the same experimental data using the simple endochronic theory with very good agreement. Ohashi et al. made the kernel function a tensor quantity. Thus, different stress components are associated with different components of the kernel function and the parameters are different for each component of the kernel function. In addition, the intrinsic time was made a function of the arc length as well as the radius of curvature of the strain path. More parameters have been introduced into the theory by this generalization. Using the method of solution of Wu and Yang [25], the endochronic constitutive equation (8.125) was applied by Wu et al. [29] to investigate the stress response to two cyclic, nonproportional strain paths in the axial–torsion strain space. The ﬁrst path involved a cyclic axial straining and unstraining following a shear prestrain, and the second path was cyclic in shear after a

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory 30

280

Axial

27 240

18 15 12 9

Stress ( or ) MPa

Stress ( or ) Kgf/mm2

24 21

200

Theory data by Ohashi et al. (1978)

160

p = 4.33 × 10–3

120

p = 8.66 × 10–3 p = 17.32 × 10–3 p = 25.98 × 10–3

80

6 3 0

439

Shear 40 0 0.0

0.2

0.4

0.6

0.8

1.0

1.2

1.4

1.6

1.8

2.0

Axial Total Strain ()%

FIGURE 8.9 Stress response to strain path of torsion followed by tension (From Wu, H.C. and Yang, R.J., Int. J. Non-Linear Mech., 18, 395, 1983. With permission from Elsevier).

prestrain in tension. Type 304 stainless steel tubular specimens were tested at constant strain-rate of 5 × 10−4 per second. The theory was capable of predicting the stress response to the two cyclic strain paths considered. Further investigation of multiaxial straining was conducted by Wu et al. [30]. Plastic strain-controlled experiments were conducted on 304 stainless steel tubular specimens. The plastic strain-control was feasible by means of a computer-aided material test system. Three in-phase plastic strain paths (a pure axial path, a pure torsional path, and an axial–torsion in-phase path) and two out-of-phase plastic-strain paths (small and large perturbations from the axial–torsion in-phase path) were studied, and the endochronic constitutive equation (8.125) was used to obtain theoretical results for the ﬁve strain paths considered. It was shown that the theory and experiment have good agreement. Furthermore, both experimental and theoretical results show that strain hardening is enhanced by out-of-phase loading. Figure 8.10(a) shows the theoretical and experimental plastic strain path of path 5, the out-of-phase path with large perturbation from the axial–torsion in-phase path. The corresponding axial stress versus plastic axial strain plot is shown in Figure 8.10(b), and the corresponding shear stress versus plastic shear strain plot is shown in Figure 8.10(c). Finally, we mention that Wu and Yeh [31] applied (8.125) to investigate the combined axial-internal pressure loading of tubular specimens and compared their results with their own experimental data. Additional work on endochronic theory and its application have been conducted by Valanis and his coworkers [32,33] and by Atluri and coworkers in numerical computation [34,35].

© 2005 by Chapman & Hall/CRC Press

440

Continuum Mechanics and Plasticity 1.2 Plastic Shear-Strain (%)

(a)

Reference Experimental D

1

E

0.8 B

0.6 0.4 0.2

C

0 0 A

–0.2 0.0

400

(b)

Experimental Endochronic

300 Axial Stress (MPa)

0.2 0.4 Plastic Axial-Strain (%)

0.6

E C

A

200 100 0 –100

D

B

–200 –300 0.0

(c)

0.2 0.4 Plastic axial-strain (%)

0.6

200

D

Shear Stress (MPa)

B 100 0

0

E A

–100

–200 –0.2

C Experimental Endochronic 0 0.2 0.4 0.6 0.8 Plastic Shear-Strain (%)

1

FIGURE 8.10 Response to zigzag plastic strain path: (a) plastic strain path, (b) axial stress, (c) shear stress (From Wu, H.C. et al., J. Eng. Mater. Technol., 108, 262, 1986. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory 8.4.6

441

The Endochronic Theory of Viscoplasticity

A general introduction of the strain-rate effect is given in Section 5.2.4. The strain-rate sensitive plasticity is also known as the viscoplasticity. Based on the ﬂow theory of plasticity, the viscoplastic effect was investigated by Perzyna [36], Phillips and Wu [37], Krempl [38], and others. The endochronic viscoplasticity provides a framework for a uniﬁed theory to discuss the constant strain-rate stress–strain curves, the creep curves, and the stress relaxation all together. In describing the viscoplastic behavior, Valanis [6] deﬁnes the intrinsic time as dζ 2 = Pijkm dεij dεkm + g2 dt2

(8.152)

where g is a material parameter. The intrinsic time given by (8.49) is a reduced version for strain-rate independent plasticity. The simple endochronic viscoplasticity was applied by Wu and his coworkers [39–41] to study the stress wave propagation for strain-rate sensitive materials. In Wu and Yip [42], the strain-rate and strain-rate history effects on the dynamic behavior of metals were investigated using the improved endochronic theory. Lin and Wu [43] further applied the theory to viscoplastic wave propagation. Furthermore, the theory was applied by Wu and Ho [44] to discuss the phenomenon of transient creep. In this subsection, we discuss the strain-rate effect for uniaxial loading following the work of [42] and creep following [44]. To obtain a more general form of the intrinsic time measure, which accounts for strain-rate, it is assumed that a spectrum of r intrinsic times exists and each intrinsic time corresponds to an internal state variable. Thus, for each intrinsic time, we write dζi2 = hi (ε p )(dε p )2 + gi (ε p )(dt)2 ,

i = 1, 2, . . . , r

(8.153)

where hi and gi are functions of dε p , and t is the real time. (8.153) can be written as gi (ε p ) 1/2 p dε , dζi = ± hi (ε p ) + p 2 (˙ε )

i = 1, 2, . . . , r

(8.154)

Introducing an average intrinsic time measure such that dζ = (dζ1 , dζ2 , . . . , dζr )

(8.155)

then, using (8.154), we obtain dζ = ±k(εp , ε˙ p )dε p

(8.156)

The function k is known as the strain-rate sensitivity function and it is a function of ε p and ε˙ p . For simplicity, we assume that k is a function of ε˙ p

© 2005 by Chapman & Hall/CRC Press

442

Continuum Mechanics and Plasticity

only, that is, dζ = k(˙ε p )|dε p |

(8.157)

This relation is the same as that proposed earlier in [39], except that we now use the plastic strain instead of the total strain. In the three-dimensional version, (8.157) is (dζ )2 = k 2 (|˙ε p |)dεp · dεp

(8.158)

Let us now consider the constant strain-rate stress–strain curves. Using (8.111), form (a) of (8.110), and (8.157), (8.109) may be integrated while holding ε˙ p constant to yield σ = σyD (1 + β1 ε p ) + (σ 0 − σyD )(1 + β1 ε p ){1 − (1 + β1 ε p )−n } + E2 ε p (8.159) where σyD =

σy k(˙ε p )

and

β1 = βk =

(8.160)

and n=

α +1 β

Et − E2 σ0

(8.161)

Note that σy is the static yield stress. The dynamic yield stress σyD , the tangent modulus Et at large εp , and the intercept of the asymptote to the stress–strain curve with the stress axis σ 0 can be measured directly from each constant strain-rate stress–strain curve (see Figure 8.5). For the sake of simplicity, we have not introduced new notations for Et and σ 0 . But these are dynamic quantities and they vary with each constant strain-rate stress–strain curve. For most materials, the constant strain-rate stress–strain curves for various strain-rates are parallel to each other at large ε p and, in this case, Et does not vary with the strain-rate. Using the method of Example 8.2, the relations in (8.161) have been obtained. The parameters β1 , n, and E2 are determined by the trial and error method so that the theoretical curve agrees with the experimental reference curve. The experimental reference curve is usually taken as the constant strain-rate stress–strain curve that has the lowest strainp rate ε˙ 0 of all the curves. The following function has been used by Lin and Wu [39] and Wu and Yip [42] to deﬁne the strain-rate sensitivity function k p

k(˙ε ) = 1 − ks log

© 2005 by Chapman & Hall/CRC Press

ε˙ p p

ε˙ 0

(8.162)

Internal Variable Theory and Endochronic Theory

443

where ks is a material parameter. Figure 8.11 shows that (1.162) can ﬁt nicely to the experimental data of Karnes and Ripperger [45] for annealed high-purity aluminum for the strain-rate range from 10−4 to 103 s−1 . The strain-rate is shown as θ˙ in the ﬁgure. From each experimental constant strain-rate stress– strain curve, we determine the dynamic yield stress σyD , and, since we know σy , k(˙ε p ) can be found from (8.160). Equation (8.159) describes a set of stress–strain curves at various constant strain-rates. By use of (8.162), the theoretical constant strain-rate stress–strain curves thus obtained are compared with the experimental curves of [45] and shown in Figure 8.12. The parameters for theoretical curves are E0 = 10 × 106 psi (6.89 × 104 MPa), σ00 = 1 × 103 psi (6.89 MPa), σy = 0.75 × 103 psi

1

k

0.8 0.6 0.4 0.2 2

4 · ·) Log(/ 0

6

8

Experiment by Karnes and Ripperger [45] · p/ · p) Theory: k = 1 – 0.1165 Log ( 0 FIGURE 8.11 Strain-rate sensitivity function k (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

00

·p = 20

Stress (MPa)

80

·p = 4000

60 40

·p =1000

·p = 500

–2

2 × 10

20 –4 s–1

2 × 10

0

0.5

1.0

1.5

2.0

Plastic Strain (%) FIGURE 8.12 Constant strain-rate stress–strain curves for aluminum (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

444

Continuum Mechanics and Plasticity

(5.17 MPa), β = 180, n = 25, and E2 = 0. We note that σ00 is the intercept of the asymptotic line with the stress axis for the reference stress–strain curve. The foregoing work is relevant to strain-hardening metallic materials such as f.c.c. metals. For materials such as mild steel, strain-softening occurs after initial yielding. However, the material switches from strain softening to strain-hardening at a strain of approximately 2%, and we shall call this type of materials strain softening–hardening materials. The ζ –z relation for this type of materials requires special attention. We use (8.110) form (c) for the strain-softening portion and form (a) for the strain-hardening portion of the material behavior, and introduce a critical intrinsic time ζcr (with the corresponding zcr ) to indicate the point of changeover from softening to hardening in a stress–strain curve. Thus, the following relations apply: dζ = f (z) = e−βs z dz

and ζ =

1 (1 − e−βs z ) βs

with βs > 0,

for z ≤ zcr (8.163)

dζ = bh eβh (z−zcr ) dz

and ζ = ζcr −

bh [1 − eβh (z−zcr ) ] βh

for z ≤ zcr (8.164)

where βs , βh , bh are material parameters. Assuming that the ζ –z relation is smooth and differentiable at the critical point, we have bh = e−βs zcr

(8.165)

Thus, bh can be calculated if βs and zcr are known. The ζ –z relation for strain softening–hardening materials is shown schematically in Figure 8.13. Using the isotropic-hardening function deﬁned by (8.163) to (8.165) and the strain-rate sensitivity function deﬁned by (8.162), (8.109) leads to the constant strain-rate stress–strain curves for mild steel shown in Figure 8.14. The plastic strain-rate is denoted by θ˙ in the ﬁgure. Theoretical results compare favorably with the experimental data of Cambell and Marsh [46] in the

cr

0

zcr

z

FIGURE 8.13 Isotropic-hardening function f for strain softening–hardening materials.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

445

70 Theory

65

Experiment by Cambell and Marsh [46]

60

= 5.0/s–1 · = 3.0 · = 0.5 · = 0.2 · = 0.02 · = 10–4

450

·

400

·

= 5.0

55

·

350 50 MPa

Stress × 103 psi

= 0.5

·

= 0.5 45

·

= 0.2

40

300

·

= 0.02 250 35

·

= 10–4/s–1 30

200 0

1

2

3

4

5

Plastic Strain (%) FIGURE 8.14 Constant strain-rate stress–strain curves for mild steel (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

range of strain-rate from 10−4 to 5 s−1 . The details of the theoretical work are reported in [42]. Wu and Yip [42] also considered the strain-rate history effect in two loading sequences: the low–high strain-rate change test sequence and the high–low strain-rate change test sequence. In the ﬁrst test sequence, the specimens

© 2005 by Chapman & Hall/CRC Press

446

Continuum Mechanics and Plasticity

were tested initially at a low prescribed constant strain-rate and tested at a higher strain-rate in the subsequent loading. In the second test sequence, the specimens were ﬁrst tested at a high strain-rate and subsequently tested at a lower strain-rate. Both strain-hardening materials and strain softening– hardening materials were investigated. Different test sequences resulted in different subsequent stress–strain behaviors. Lin and Wu [43] used a nonlinear form of (8.162) to describe the strain-rate sensitive behavior of α-titanium. The intrinsic time deﬁned by (8.158) is applicable to describing constant strain-rate stress–strain curves as previously shown. In the uniﬁed theory, (8.158) is combined with (8.152) to yield (dz)2 =

dζ f (ζ )

2

+ g2 dt2

(8.166)

where (dζ )2 = k 2 (|˙ε p |)dε p · dε p

and

k(|˙ε p |) = 1 − ks log

|˙εp | |˙ε p |0

(8.167)

The intrinsic time expressed by (8.166) and (8.167) provides a versatile deﬁnition of intrinsic time. In this way, the strain-rate sensitive plasticity (the rate dependence) can be accounted for by the function k(|˙εp |), and (8.167) shows that the accumulation of ζ is strain-rate dependent. Creep or stress relaxation behavior (the time dependence) is accounted for by the function g. Although both rate dependence and time dependence are time-dependent behaviors, it is convenient to use these terminologies. A ﬂow theory of viscoplasticity can be derived from the endochronic viscoplasticity equations. The method of derivation and the resulting equations are the same as those presented in Section 8.4.4, except that the yield stress is replaced by the dynamic yield stress. The dynamic yield stress is deﬁned by (8.160) through the strain-rate sensitivity function k. The ﬂow rule remains the same as in (8.97), which is dεp =

(σ − α) dz σy

(8.168)

but the yield criterion is now

(σ − α) · (σ − α) =

σy f (z)

2

k

with dζ 2 = 0

(8.169)

or dζ 2 = 0

© 2005 by Chapman & Hall/CRC Press

(8.170)

Internal Variable Theory and Endochronic Theory

447

The function k describes the strain-rate sensitivity of the dynamic loading surface so that σy /k is the size of the constant strain-rate dynamic loading surface, which is also known as the SCISR (surface of constant inelastic strainrate) — an acronym introduced by Robinson [47]. The function f denotes the size of the SCISR due to isotropic hardening and α denotes the location of the center of the SCISR. The distortion of the yield and loading surfaces is not described by (8.169). That subject has been discussed by Wu et al. [48] and Wu and Lu [49]. In the case of time-dependent deformation process (creep or stress relaxation), g = 0; (8.167) and (8.168) may be substituted into (8.166) to obtain dz2 = k 2 (|˙ε p |)

|σ − α|2 2 dz + g2 dt2 (σy f )2

(8.171)

or dz =

g 1 − k 2 (|σ − α|2 /(σy f )2 )

dt

(8.172)

Note that since dz > 0 and dt > 0, it must be that g > 0. Acreep test is preceded by a constant strain-rate test. During this stage of plastic deformation, the stress point is on the yield surface which from (8.169) is σ f (z) σ − α = y k

or

1 − k2

|σ − α|2 =0 (σy f )2

(8.173)

However, since the stress point in the stress space stays at the same point but the back stress increases during creep as experimentally observed by Wu and Ho [50] for annealed 304 stainless steel (there may also be isotropic hardening for other materials), the stress point, which is on the SCISR when creep begins, falls back into the “elastic region” of that SCISR as the SCISR moves during creep. In the case of stress relaxation, the stress point also falls back into the “elastic region” of the SCISR as the stress level reduces. Therefore, during time-dependent inelastic behavior 1 − k2

|σ − α|2 = 0 (σy f )2

(8.174)

In an effort to unify the deﬁnition of intrinsic time for both plastic deformation and time-dependent inelastic behavior, the function g must reduce to zero in the case of plastic deformation. To this end, the following form of g has been

© 2005 by Chapman & Hall/CRC Press

448

Continuum Mechanics and Plasticity

found to be satisfactory g = B 1 − k2

|σ − α|2 (σy f )2

(8.175)

where B is a scaling function. Substituting (8.175) into (8.172), the intrinsic time for time-dependent inelastic behavior is now given by dz = B dt

(8.176)

and the time-dependent inelastic strain (creep) may be found from (8.168) as dσ (σ − α) = B dt 2µ0 σy

dεp = de −

(8.177)

which is rewritten as

dσ = 2µ0

(σ − α) de − B dt σy

(8.178)

In the rate form, (8.178) is

σ˙ = 2µ0

(σ − α) e˙ − B σy

(8.179)

Creep and stress relaxation are now discussed separately. In the case of creep, the stress holds constant, that is, σ˙ = 0, and the creep strain-rate (˙εp )c equals the total strain-rate. Therefore, from (8.179) (˙εp )c = e˙ =

(σ − α) B σy

(8.180)

The form of the scaling function B is now investigated. Miller [51] suggested that the creep rate is a function of kinematic and isotropic hardenings and proposed the expression p

(˙ε )c = ϕ

σ − α R

(8.181)

where R denotes isotropic hardening; σ is the hold stress; and ϕ is a nonlinear function to be further discussed. Thus, during the creep process, both kinematic and isotropic hardenings are active. The form of (8.181) encompasses the experimental observations that both isotropic and kinematic hardenings can be important factors in creep [50]. This equation is, therefore,

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

449

used in this chapter. In classical creep theories and uniﬁed viscoplasticity theories, the power, the exponential, and the hyperbolic sine functions are usually used to provide a description of creep strain. Of these functional forms, the power form has been broadly used because of its numerical simplicity. This function is now used in this writing, so that B=

bσy |σ − α|

k|σ − α| σy f

m (8.182)

where b and m are material parameters. Finally by substituting (8.182) into (8.180), the creep strain-rate is obtained as

k|σ − α| (˙εp )c = b σy f

m

(σ − α) |σ − α|

(8.183)

which is a specials case of (8.181). At the very beginning when creep is about to occur, the stress is still on the loading surface (SCISR) so that, from (8.169), |σ −α| = (σy f )/k, g = 0, and (8.183) does not apply yet. However, only a small perturbation so that |σ −α| < (σy f )/k would start the creep process and make (8.183) applicable. Since the perturbation is small, |σ − α| ≈ (σy f )/k, so that (˙εp )c = b. Therefore, b may be identiﬁed as the initial creep strain-rate. During the process of stress relaxation, the total strain increment de = 0 so that, by use of (8.179), the rate of stress relaxation is σ˙ = −2µ0 B

σ − α σy

(8.184)

Wu and Ho [44] applied the foregoing theory to describe their own experimental results for AISI type 304 stainless steel. Isotropic hardening is insigniﬁcant for this material [52]. It has been shown in [44] that the viscoplastic endochronic constitutive equation is capable of describing the inelastic behavior of this rate-sensitive metal for a variety of loading histories. The features include combined isotropic–kinematic hardening, rate sensitivity of plastic deformation, creep, and stress relaxation. In particular, the creep curves with a constant strain-rate preloading stage previously shown in Figure 5.13 are well predicted. In addition, they found that (1) meaningful results of transient creep can be obtained only from creep tests with a carefully controlled constant strain-rate preloading stage; (2) a correlation between constant strain-rate and constant stress-rate stress–strain curves can be achieved by means of the viscoplastic endochronic constitutive equations; (3) with the same strain-rate in the elastic region, the stress–strain curve of constant stress-rate is stiffer than that of constant strain-rate; (4) a correlation between creep with constant strain-rate and constant stress-rate preloadings can be achieved by means of the viscoplastic endochronic constitutive equations;

© 2005 by Chapman & Hall/CRC Press

450

Continuum Mechanics and Plasticity

and (5) the initial creep rate is a continuation of the strain-rate of preloading and the creep curves are noticeably inﬂuenced by the initial creep rate.

References 1. Valanis, K.C., The viscoelastic potential and its thermodynamic foundation, Iowa State Univ., ERI Report 52, 1967, J. Math. Phys., 48, 262, 1968. 2. Valanis, K.C., Irreversibility and existence of entropy, Int. J. Nonlinear Mech., 6, 337, 1971. 3. Valanis, K.C., Proper tensorial formulation of the internal variable theory, The endochronic time spectrum, Arch. Mech., 29, 173, 1977. 4. Valanis, K.C., A gradient theory of internal variables, Acta Mech., 116, 1, 1996. 5. Valanis, K.C., Irreversible Thermodynamics of Continuous Media, Springer-Verlag, Udine, 1971. 6. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 7. Valanis, K.C., Fundamental consequences of a new intrinsic time measureplasticity as a limit of the endochronic theory, Arch. Mech. 32, 171, 1980. 8. Callen, H.B., Thermodynamics, John Wiley & Sons, New York, 1960, 15. 9. Coleman, B. and Gurtin, M., Thermodynamics of internal state variables, J. Chem. Phys., 47, 599, 1967. 10. Ilyushin, A.A., On the relation between stresses and small strains in continuum mechanics, Prikl. Mat. Mekh., 18, 641, 1954 (in Russian). 11. Pipkin, A.C. and Rivlin, R.S., Mechanics of rate-independent materials, J. Appl. Math. Phys. (ZAMP), 16, 313, 1965. 12. Valanis, K.C. and Wu, H.C., Endochronic representation of cyclic creep and relaxation of metals, J. Appl. Mech., 42, 67, 1975. 13. Wu, H.C. and Lin, H.C., Combined plastic waves in a thin-walled tube, Int. J. Solids Struct., 10, 903, 1974. 14. Lin, H.C. and Wu, H.C., Strain-rate effect in the endochronic theory of viscoplasticity, J. Appl. Mech., 43, 92, 1976. 15. Kosinski, W. and Wu, H.C., On steady viscoplastic waves. Endochronic theory, Bull. L’Acad. Polon. Sci., Ser. Sci. Tech., 26, 109, 1978. 16. Wu, H.C. and Yip, M.C., Finite difference solution for the uniaxial endochronic viscoplastic wave problem, J. Appl. Mech., 45, 221, 1978. 17. Jao, S.Y., Arora, J.S., and Wu, H.C., An optimization approach for materialconstant determination for the endochronic constitutive model, Comput. Mech., 8, 25, 1991. 18. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 19. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 20. Prager, W., The theory of plasticity: a survey of recent achievements (James Clayton Lecture), Proc. Inst. Mech. Eng., 169, 41, 1955.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

451

21. Ziegler, H., A modiﬁcation of Prager’s hardening rule, Quart. Appl. Math., 17, 55, 1959. 22. Wu, H.C. and Yip, M.C., Endochronic description of cyclic hardening behavior for metallic materials, J. Eng. Mater. Technol., 103, 212, 1981. 23. Lamba, H.S. and Sidebottom, O.M., Proportional biaxial cyclic hardening of annealed oxygen-free high-conductivity copper, J. Test. Evaluation, 6, 260, 1978. 24. Wu, H.C., Aboutorabi, M.R., and Chen, P.C.T., Cyclic torsion of a circular cylinder and its residual stress distribution, J. Eng. Mater. Technol., 107, 48, 1985. 25. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 26. Ohashi, Y., Tokuda, M., and Tanaka, Y., Precise experimental results on plastic behavior of brass under complex loading, Bull. De L’Acad. Polon. Des Sci., Ser. Sci. Tech., 26, 261, 1978. 27. Ohashi, Y., Tokuda, M., Mitake, T., Kurita, Y., and Suzuki, T., Stress–strain relation of integral type for deformation of brass along strain trajectories consisting of three normal straight branches, Archs. Mech., 32, 125, 1980. 28. Ohashi, Y., Tokuda, M., Suzuki, T., and Kurita, Y., Stress–strain relation of brass for the plastic deformation along bi-linear strain trajectories with various corner angles, Bull. Japan. Soc. Mech. Eng., 24, 1909, 1981. 29. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 30. Wu, H.C., Yao, J.C., and Chu, S.C., Investigation of endochronic constitutive equation subjected to plastic strain-controlled axial-torsional deformation, J. Eng. Mater. Technol., 108, 262, 1986. 31. Wu, H.C. and Yeh, W.C., Further veriﬁcation of endochronic theory under biaxial load, J. Eng. Mater. Technol., 111, 115, 1989. 32. Valanis, K.C. and Fan, J., Endochronic analysis of cyclic elastoplastic strain ﬁelds in a notched plate, J. Appl. Mech., 50, 789, 1983. 33. Valanis, K.C. and Lee, C.F., Endochronic theory of cyclic plasticity with application, J. Appl. Mech., 51, 367, 1984. 34. Watanabe, O. and Atluri, S.N., A new endochronic approach to computational elastoplasticity: example of a cyclically loaded cracked plate, J. Appl. Mech., 52, 857, 1985. 35. Watanabe, O. and Atluri, S.N., Internal time, general internal variable, and multi-yield-surface theories of plasticity and creep: a uniﬁcation of concepts, Int. J. Plasticity, 2, 37, 1986. 36. Perzyna, P., The constitutive equations for rate sensitive plastic materials, Quart. Appl. Math., 20, 321, 1963. 37. Phillips, A. and Wu, H.C., A theory of viscoplasticity, Int. J. Solids Struct., 9, 15, 1973. 38. Krempl, E., Models of viscoplasticity. Some comments on equilibrium (back) stress and drag stress, Acta Mech., 69, 25, 1987. 39. Lin, H.C. and Wu, H.C., Strain-rate effect in the endochronic theory of viscoplasticity, J. Appl. Mech., 43, 92, 1976. 40. Wu, H.C. and Yip, M.C., Finite difference solution for the uniaxial endochronic viscoplastic wave problem, J. Appl. Mech., 45, 221, 1978.

© 2005 by Chapman & Hall/CRC Press

452

Continuum Mechanics and Plasticity

41. Kosinski, W. and Wu, H.C., On steady viscoplastic waves. Endochronic theory, Bull. L’Acad. Polon. Scien., Ser. Sci. Tech., 26, 109, 1978. 42. Wu, H.C. and Yip, M.C., Strain rate and strain rate history effects on the dynamic behavior of metallic materials, Int. J. Solids Struct., 16, 515, 1980. 43. Lin, H.C. and Wu, H.C., On the rate-dependent endochronic theory of viscoplasticity and its application to plastic-wave propagation, Int. J. Solids Struct., 19, 587, 1983. 44. Wu, H.C. and Ho, C.C., An investigation of transient creep by means of endochronic viscoplasticity and experiment, J. Eng. Mater. Technol., 117, 260, 1995. 45. Karnes, C.H. and Ripperger, E.A., Strain-rate effect in cold worked high-purity aluminum, J. Mech. Phys. Solids, 14, 75, 1966. 46. Cambell, J.D. and Marsh, K.J., The effect of strain-rate on the post-yield ﬂow of mild steel, J. Mech. Phys. Solids, 11, 49, 1963. 47. Robinson, D.N., On thermomechanical testing in support of constitutive equation development for high temperature alloys, NASA CR 174879, 1985. 48. Wu, H.C., Hong, H.K., and Lu, J.K., An endochronic theory accounted for deformation induced anisotropy, Int. J. Plasticity, 11, 145, 1995. 49. Wu, H.C. and Lu, J.K., Further development and application of an endochronic theory accounted for deformation induced anisotrophy, Acta Mech., 109, 11, 1995. 50. Wu, H.C. and Ho, C.C., Strain hardening of annealed 304 stainless steel by creep, J. Eng. Mater. Technol., 115, 345, 1993. 51. Miller, A.K., An inelastic constitutive model for monotonic, cyclic, and creep deformation, J. Eng. Mater. Technol., 98, 97, 1976. 52. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991.

Problems (1) Derive (8.66) and (8.67). (2) Derive (8.71) and (8.72). (3) In the simple endochronic theory, if in the one-dimensional straining the intrinsic time is deﬁned by dζ = ±k dε, where k is a constant, plot the ε versus ζ relation for straining followed by unstraining. (4) For a thin-walled tube made of an initially isotropic material subjected to combined axial–torsion, determine k1 and k2 in the expression dζ 2 = k12 (dεp )2 + k22 (dηp )2 , where ζ is intrinsic time and ηp is the plastic part of the tensorial shear strain. (5) Show that the solution of (8.90) is given by (8.91) and (8.92), if k1 = 1. (6) We consider here the kernel function ξ(z) of the deviatoric constitutive equation (8.82). In Example 8.2, the kernel function is given by two exponential terms. Consider now the case that the kernel function consists of n number of

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

453

(b)

(a)

0

60°

FIGURE 8.15 (a) Figure of Problem (8), (b) Figure of Problem (9).

exponential terms, show that in the case of k1 ≈ 1, the deviatoric stress is

σ = 2µ0 where ρ(z) = δ(z) +

z 0

ξ(z − z )

n−1 s

z de dQ dz = 2µ ρ(z − z ) dz 0

dz dz 0

Rs e−αs z + R0 .

(7) In the strain controlled cyclic loading discussed in Section 8.4.5.2, the amplitude of the total strain is kept constant throughout the test. The amplitude of the plastic strain ˜εp becomes constant at stable condition. Let ζ˜ denote the change in ζ in 41 -cycle at the stable condition and the corresponding change in z is ˜z. Show that, if Form (b) of (8.110) is used for the f function, then when z is large ζ˜ /C = ˜z = constant. Show that the cyclic stress–strain curve is σ = σ 0 − (σ 0 − Cσy )

2e−2α˜z 1 + e−2α˜z

+ E2 ε p

(8) In a strain-controlled combined tension–torsion test of a tubular specimen, if the strain-path is linear shown in Figure 8.15(a), use the endochronic constitutive equation to determine the corresponding stress-path. (9) In a stress-controlled combined tension–torsion test of a tubular specimen, consider the tor-ten path shown in Figure 8.15(b). Use the endochronic constitutive equation to determine the corresponding strain-path. Plot the strain-path. (10) In the constant strain-rate uniaxial stress test, if the test is conducted at a low strain-rate into the plastic strain range and then changed to a higher constant strain-rate, what happens to the stress–strain curve?

© 2005 by Chapman & Hall/CRC Press

9 Topics in Endochronic Plasticity

9.1

Introduction

The endochronic theory of plasticity presented in Chapter 8 is further developed in this chapter and applied to investigate topics such as anisotropic plasticity, ﬁnite plastic deformation, engineering materials with plastic volumetric deformation, and damage mechanics. It is seen that the endochronic theory is versatile and is applicable to a wide range of engineering materials.

9.2

An Endochronic Theory of Anisotropic Plasticity

Material anisotropy is a signiﬁcant factor affecting metal forming, and it is of special importance in the case of sheet metals. The anisotropic properties of sheet metals are discussed in Chapter 10 from the viewpoint of the ﬂow theory of plasticity. A general theory of anisotropic plasticity is developed in Chapter 11 using a convected coordinate system. In this section, we discuss the anisotropic plastic behaviors of metals using a endochronic plasticity. We discuss the topic of deformation induced anisotropy and develop an endochronic theory for anisotropic sheet metals.

9.2.1

An Endochronic Theory Accounting for Deformation Induced Anisotropy

In the endochronic theory, the free energy function is from (8.63) given by = 12 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr

(9.1)

The constitutive equation and the evolution equations are from (8.51) and (8.57) σ=

∂ ∂ε

and

r ∂ r dq + b · = 0, ∂qr dz

r = 1, 2, . . . , n

(9.2) 455

© 2005 by Chapman & Hall/CRC Press

456

Continuum Mechanics and Plasticity

where A, Br , Cr , and br are isotropic fourth-rank constant tensors; σ, ε, and qr are symmetric tensors. By use of (9.1) and (9.2), the constitutive equation becomes σkk = 3A0 εkk + σij = A2 eij +

3 Br0 qrkk

r

(9.3)

Br2 pijr

r

To consider deformation induced anisotropy, the evolution of qr must depend on the strain path. This may be achieved by having an anisotropic br . Following Wu and Yeh [1], we deﬁne a strain path with reference to a coordinate system. Thus, we may talk about the normal strain and the shear strain. The internal structure of a material changes differently when it is under normal strain and under shear strain. Hence, qr11 evolves differently than qr12 . We assume that qrij is symmetric and write its components in a matrix form as [qr ] = [qr11 , qr22 , qr33 , qr23 , qr13 , qr12 ]T

(9.4)

We assume further that, in the internal structure, no coupled effect exists either between shear and normal components or among shear components. Then, tensor brijkm is of the following form:

br1 br 2 r b2 r [b ] = 0 0

br2

br2

0

0

br1

br2

0

0

br2 0

br1 0

0 br3

0

0

0

0

0

0

0

0

0 br3

0 0 0 0

0

0

br3

(9.5)

The matrix in (9.5) is obtained by considering symmetry during permutation of 1, 2, and 3. We further have br1111 = br2222 = br3333 = br1 , br2323 = br1313 = br1212 = br3 , other brijkm = 0 br1122 = br1133 = br2233 = br3311 = · · · = br2 ,

(9.6)

We now consider the evolution of qr . Using (9.1), we obtain the following expression ∂ = Br1 εkk δij + Br2 εij + C1r qrkk δij + C2r qrij ∂qrij

© 2005 by Chapman & Hall/CRC Press

(9.7)

Topics in Endochronic Plasticity

457

On the other hand, we have r (b1 − br2 )˙qr11 + br2 q˙ rkk br1 q˙ r11 + br2 q˙ r22 + br2 q˙ r33 br q˙ r + br q˙ r + br q˙ r (br − br )˙qr + br q˙ r 1 2 11 1 22 2 33 2 22 2 kk r r r rq r + br q r r )˙ r + br q r ˙ ˙ ˙ b + b (b − b q q 2 11 2 22 1 33 2 33 2 ˙ kk 1 = br · q˙ r = r r r r b3 q˙ 23 b3 q˙ 23 br3 q˙ r13 br3 q˙ r13

br3 q˙ r12

(9.8)

br3 q˙ r12

Substituting (9.7) and (9.8) into the second equation of (9.2), we obtain the evolution equations for the cases of i = j and i = j. Thus, the governing equations are summarized below. The hydrostatic equations are σkk = 3A0 εkk + 3

Br0 qrkk

r

Br0 εkk

+ C0r qrkk

+ br0

(9.9)

dqrkk =0 dz

and the deviatoric equations are σij = A2 eij +

Br2 pijr

r

Br2 eij + C2r pijr + (br1 − br2 ) Br2 eij + C2r pijr + br3

dpijr dz dpijr dz

= 0,

i=j

= 0,

i = j

(9.10)

It is assumed that the material is plastically incompressible so that only the deviatoric part of the constitutive equation is of further interest. The evolution equations in (9.10) for i = j and i = j can be solved separately to yield expressions for piri (i not summed) and pijr , which are then substituted into the ﬁrst equation of (9.10) to yield σii

z 2 2 e−ρr (z−z ) ei i (z )dz , r C 0 2 r Br Br z 2 2 A2 eij − e−βr (z−z ) eij (z )dz , r C 0 2 r

= A2 ei i −

σij =

Br Br

i not summed (9.11) i = j

where ρr =

© 2005 by Chapman & Hall/CRC Press

C2r , br1 − br2

βr =

C2r br3

(9.12)

458

Continuum Mechanics and Plasticity

By use of Laplace transformation as in Section 8.4.3, (9.11) may be rewritten in terms of plastic strain as

p

σij

=

σy

deij dz

+

z 0

p

de λijkm (z − z ) km dz dz

(9.13)

where

µ

[λ] =

µ

0 µ

ν

ν

0

µ(z) = with

µr e−mr z + µ1

r

ν(z) =

νr e−nr z + ν1

(9.14)

r

ν

in which µr , mr , νr , and nr are material constants of the kernel functions µ(z) and ν(z). Note that in the case of br1 = br2 + br3 , we ﬁnd ρr = βr , which leads to µ(z) = ν(z). Thus, the following endochronic equation for the isotropic rate of kinematic hardening is recovered:

p

σij = σy

deij

+

dz

z 0

p

µ(z − z )

deij dz

dz

(9.15)

We note that the anisotropic form (9.13) is the same as that used by Ohashi and his coworkers [2,3]. Let us further consider the anisotropic endochronic equation (9.13) and, following Wu et al. [4], establish a relation between the deﬁnition of the intrinsic time and the form of the yield function. In (9.13), the back stress is αij =

z 0

p

de λijkm (z − z ) km dz dz

(9.16)

Thus, (9.13) is written as p

σij

− αij =

σy

deij dz

p

=

σy

f (z)

deij dζ

(9.17)

resulting in the following ﬂow rule p

deij =

1 (σ − αij ) dz σy ij

(9.18)

Deﬁne the intrinsic time as dζ 2 = dep · K · dep

© 2005 by Chapman & Hall/CRC Press

(9.19)

Topics in Endochronic Plasticity

459

in which K is a fourth-rank tensor. Then, by using (9.18), (9.19) becomes dζ 2 = (σ − α)

dζ dζ · K · (σ − α) σy f σy f

(9.20)

or [(σ − α) · K · (σ − α) − (σy f )2 ]dζ 2 = 0

(9.21)

Therefore, Either (σ − α) · K · (σ − α) = (σy f )2 or

dζ = 0

with dζ 2 = 0

elastic behavior

(9.22)

The ﬁrst equation of (9.22) is the yield criterion of this anisotropic version of the endochronic plasticity and the second equation of (9.22) describes the elastic behavior, which may be seen from (9.19) due to the positive deﬁniteness of K. The condition dζ = 0 leads to the elastic constitutive equation as in (8.104). p From (9.19), due to the symmetry of deij , Kijkm enjoys the following symmetry: p

p

p

p

deij Kijkm dekm = dekm Kkmij deij , Kijkm = Kkmij = Kijmk

p

p

p

p

deij Kijkm dekm = deij Kijmk demk ,

(9.23)

The number of independent components of K is reduced from 81 to 21. In most previous investigations, K was assumed to be isotropic throughout the course of deformation for mathematical simplicity. This assumption is now relaxed so that K depends on the direction of loading. Equation (9.19) simply asserts that the rate of accumulation of the intrinsic time ζ is not the same when the material is subjected to shear or subjected to tension. However, K is initially isotropic for initially isotropic materials. In which case, the ﬁrst equation of (9.22) reduces to the Mises yield criterion. Equation (9.22) represents a distortion from the Mises yield criterion due to the presence of K. This criterion may be used for the initial as well as the subsequent yielding. In particular, (9.22) can accommodate the idea that the initial yield surface is of the type of Mises, but the subsequent yield surfaces are obtained by the compression and stretching of the Mises yield surface. It should also be pointed out that while the plastic strain increment is still given by (9.18) in this modiﬁed theory, this tensor is no longer normal to the yield surface when K is not isotropic. An important point to make here is that a formal link between the deﬁnition of intrinsic time and the form of the yield function has been established. The deﬁnition of intrinsic time directly affects the form of the yield function, so that

© 2005 by Chapman & Hall/CRC Press

460

Continuum Mechanics and Plasticity

the intrinsic time deﬁned by (9.19) leads to a yield function deﬁned by (9.22). On the other hand, a slightly different deﬁnition of intrinsic time, such as dζ 2 = dεp · K · dεp + tr(L · dεp ) dζ

(9.24)

would lead to a yield function given by (σ − α) · K · (σ − α) + σy f (z) tr[L · (σ − α)] = (σy f (z))2

(9.25)

where L is a material tensor. Explicit equations can be obtained from the theory of this subsection in the case of axial–torsion loading of a thin-walled tubular specimen. Since the material is assumed to be plastically incompressible and the cylindrical coordinates (r, θ , z) are used in this discussion, the conditions p p p p p dεzz + dεrr + dεθθ = 0 and dεrr = dεθθ apply. The latter condition is a good approximation in the case of small plastic deformation, but it is not so when plastic deformation is large; see Wu et al. [5] for further discussion. The matrices of the deviatoric stress σ , the back stress α, and the plastic strain increment dεp are −σ

3 [σ ] = 0 0 −dε p 2 [dεp ] = 0 0

0 −σ 3 τ

−α

0

τ , 2σ 3 0

−dε p 2 dηp

3 [α] = 0 0

zz

0 −αzz 3 αθz

0

αθz , 2αzz 3

0 p dη dε p

(9.26)

which may also be written as column vectors as

−σ 3 2σ , [σ ] = 3 τ

−αzz 3 2α [α] = zz , 3 αθz

−dε p

2 [dεp ] = dε p

(9.27)

dηp

Then, the fourth-rank tensor K is given by the square matrix

K11 [K] = K12 K13

© 2005 by Chapman & Hall/CRC Press

K12 K22 K23

K13 K23 K33

(9.28)

Topics in Endochronic Plasticity

461

Substituting (9.27) and (9.28) into (9.19), we obtain dζ 2 = dεp · K · dεp = K1 (dε p )2 + 2K3 (dε p )(dηp ) + K2 (dηp )2

(9.29)

where K1 =

K11 − K12 + K22 , 4

K2 = K33 ,

K3 =

1 (2K23 − K13 ) 2

(9.30)

and, by using (9.18), the yield function (9.22) becomes 4 9 K1 (σ

− αzz )2 + 43 K3 (σ − αzz )(τ − αθz ) + K2 (τ − αθz )2 = (σy f (z))2

(9.31)

It can be seen from (9.31) that the yield function is an ellipse in the σ versus τ space. As plastic deformation occurs, the ellipse will change its shape, depending on the values of K1 and K2 , when the semimajor and semiminor axes change their lengths. At the same time, isotropic hardening takes place according to function f (z) and the ellipse translates according to the magnitude of the back stress α. In addition, rotation of the yield surface occurs according to the value of 2K3 . Therefore, the major features of subsequent yield surfaces as observed experimentally by Phillips and Tang [6] and Wu and Yeh [7] can all be described. From the experimental results of Phillips and his coworkers, the initial value of K3 is zero. Then by comparing equation (9.31) with the Mises yield criterion, the initial values of K1 and K2 are determined to be 3/2 and 2, respectively. Wu and Lu [8] have established a procedure to determine the metric of the anisotropic intrinsic time using information related to the yield surface of 304 stainless steel.

9.2.2

An Endochronic Theory for Anisotropic Sheet Metals

The contents of this section were initially presented by Wu and Hong [9] and are reproduced here with permission from Elsevier. In the Helmholtz formulation, the free energy is =

1 r A (εij − qrij )(εkm − qrkm ) 2 r ijkm

(9.32)

where Arijkm are constants. For a rolled metal sheet, let x denote the rolling direction (RD), y the transverse direction (TD), and z the normal direction (ND). The nonzero strain components are εx , εy , εxy , and εz . No energy is stored due to εz . Thus, (9.32) reduces to =

1 r [A (εx − qrx )2 + Br (εy − qry )2 + 2Dr (εxy − qrxy )2 2 r + 2Cr (εx − qrx )(εy − qry )]

© 2005 by Chapman & Hall/CRC Press

(9.33)

462

Continuum Mechanics and Plasticity

where Ar , Br , Cr , and Dr are constants. The stress components are

σx = σy = σxy =

∂ = [Ar (εx − qrx ) + Cr (εy − qry )] ∂εx r

(9.34a)

∂ = [Br (εy − qry ) + Cr (εx − qrx )] ∂εy r

(9.34b)

∂ = [Dr (εxy − qrxy )] ∂εxy r

(9.34c)

and the evolution equations for the internal variables are from (8.57): dqrkm ∂ r =0 + b ijkm ∂qrij dz

(r not summed)

(9.35)

In the rolled sheet metal, the components of internal variables are (qrx , qry , qrxy ) and it is assumed that there are no coupling effects among these components, so that the dissipation tensor has the following form

brx

[br ] = 0 0

0 bry 0

0 0 brxy

(9.36)

Using (9.33) and (9.36), (9.35) reduces to dqrx + Pr qrx + U r qry = Pr εx + U r εy dz dqry + Qr qry + V r qrx = Qr εy + V r εx dz dqrxy + Rr qrxy = Rr εxy dz

(9.37a) (9.37b) (9.37c)

where

Pr =

Ar , brx

Ur =

© 2005 by Chapman & Hall/CRC Press

Cr , brx

Qr =

Br , bry

Vr =

Cr , bry

Rr =

Dr brxy

(9.38)

Topics in Endochronic Plasticity

463

Note that (9.37a,b) are coupled in qrx and qry . A standard procedure may be used to decouple the equations. The resulting equations are d¯qrx ˜ r εy + λr1 q¯ rx = C˜ r εx + D dz d¯qry + λr2 q¯ ry = E˜ r εx + F˜ r εy dz

(9.39a) (9.39b)

r r

r where λr1 and λr2 are eigenvalues of the matrix VP r U Qr . Note that since U = 0 r r r and V = 0, there are always two real eigenvalues. q¯ x and q¯ y are related to qrx and qry through the eigenvectors of the matrix by the following relations qrx = U r (¯qrx + q¯ ry ),

qry = (−Pr + λr1 )¯qrx + (−Pr + λr2 )¯qry

(9.40)

and [−(Pr )2 + λr2 Pr − Pr V r + λr1 V r ] U r (λr2 − λr1 ) [−Pr U r + λr2 U r − Pr Qr + λr1 Qr ] ˜r = D U r (λr2 − λr1 ) (U r Pr + U r V r ) E˜ r = U r (λr2 − λr1 ) C˜ r =

(9.41)

[(U r )2 + U r Qr ] F˜ r = U r (λr2 − λr1 ) Note that (9.39a,b) are now decoupled in q¯ rx and q¯ ry . These equations may be integrated with results substituted into (9.40) to obtain qrx = U r

z 0

r

+U qry

z

r

= (−P

0 r

˜ r εy (z )]dz e−λ1 (z−z ) [C˜ r εx (z ) + D r e−λ2 (z−z ) [E˜ r εx (z ) + F˜ r εy (z )]dz

+ λr1 )

z

0

r ˜ r εy (z )]dz e−λ1 (z−z ) [C˜ r εx (z ) + D

+ (−Pr + λr2 )

(9.42a)

0

z

e−λ2 (z−z ) [E˜ r εx (z ) + F˜ r εy (z )]dz r

(9.42b)

Also, (9.37c) may be integrated to yield qrxy = Rr

© 2005 by Chapman & Hall/CRC Press

z 0

e−R (z−z ) εxy (z )dz r

(9.42c)

464

Continuum Mechanics and Plasticity

with qrx (0) = qry (0) = qrxy (0) = 0. By substitution of (9.42) into (9.34) and by use of integration by parts, the following expressions are found

dε dεx r ˜ r y dz e−λ1 (z−z ) C˜ r + D dz dz 0 r

z dεy dεx r Nr (9.43a) e−λ2 (z−z ) E˜ r + F˜ r dz + dz dz 0 r

σx = Y1 εx (z) + Y2 εy (z) +

Mr

dε dεx r ˜ r y dz e−λ1 (z−z ) C˜ r + D dz dz 0 r

z (9.43b) r −λr2 (z−z ) ˜ r dεx r dεy ˜ L E dz e +F + dz dz 0 r

σy = Y3 εy (z) + Y4 εx (z) +

σxy =

z

D

r

z

Kr

z

r 0

r dεxy e−R (z−z ) dz dz

(9.43c)

where

˜r − Mr C˜ r − N r E˜ r , Y2 = C − Mr D N r F˜ r r r r r ˜r − Y3 = B − Kr D Lr F˜ r , Y4 = C − K r C˜ r − Lr E˜ r r r r r A= Ar , B = Br , C = Cr ,

Y1 = A −

r

1 = r Ar U r + Cr (−Pr + λr1 ) , λ1

1 r K = r Cr U r + Br (−Pr + λr1 ) , λ1

Mr

r

r

1 = r Ar U r + Cr (−Pr + λr2 ) λ2

1 r r r L = r C U + Br (−Pr + λr2 ) λ2 (9.44)

Nr

Note that all quantities given in (9.44) are constants. A special case of (9.43) is used to derive the following equations

dεy dεx G(z − z ) (H + F) + H dz dz dz 0

z dεy dεx σy = K −3/2 G(z − z ) (G + H) + H dz dz dz 0

z M dεxy σxy = K −3/2 dz Gxy (z − z ) N dz 0 σx = K −3/2

© 2005 by Chapman & Hall/CRC Press

z

(9.45)

Topics in Endochronic Plasticity where

465

r G(z) = Gr e−λ z r r −λrxy z Gxy (z) = Gxy e r

K = 23 (F + G + H)

Gr = 1 r r with Gxy (0) = Gxy =1

with G(0) =

(9.46)

r

and

M = (H + F)(G + H) − H 2

Constitutive equations (9.45) are suitable for use in sheet metals. These are expressions for the stress components in terms of the histories of the total r , λr , and strain components εx , εy , and εxy . In the equations, E, F, G, H, Gr , Gxy r λxy are constants with r = 1, . . . , n. The derivation of (9.45) is given in [9]. It is now desirable to express the stress in terms of the histories of plastic p p p strain components εx , εy , and εxy so that p z p dε dε y x σx = K −3/2 ρ(z − z ) (H + F) + H dz dz dz 0 p z p dεy dεx −3/2 (9.47) σy = K ρ(z − z ) (G + H) + H dz dz dz 0 z p M dε x dz σxy = K −3/2 ρxy (z − z ) N dz 0 The forms of expressions in the square brackets on the right-hand side of (9.45) and (9.47) are assumed to be the same. These forms are established based on plastic deformation for sheet metals, which is further discussed in Chapter 10. The coefﬁcients F, G, H, M, and N are those of the yield function initially proposed by Hill [10]. The kernel functions ρ(z) and ρxy (z) can be determined from knowledge of G(z) and Gxy (z) using the method of Laplace transformation discussed in Section 8.4.3. Omitting the details of derivation, which may be found in [9], the kernel functions are ρ(z) = δ(z) + ρ1 (z)

with ρ1 (z) =

n−1

Rr e−µr z

r=1 n−1

ρxy (z) = δ(z) + ρxy1 (z)

with ρxy1 (z) =

(9.48) r Rxy e−µxyr z

r=1

where µr , and µxyr are positive constants. Substituting (9.48) into (9.47), the constitutive equations for sheet metals may be obtained: Rr ,

r , Rxy

σx = K −3/2

p

p

dεy dεx (H + F) +H dz dz

+ K −3/2

© 2005 by Chapman & Hall/CRC Press

z

0

p

p

dεy dεx ρ1 (z − z ) (H + F) + H dz dz

dz

(9.49a)

466

Continuum Mechanics and Plasticity σy = K

p

z

Denoting

p

dεy

p

dεx ρ1 (z − z ) (G + H) + H +K dz dz 0 z p M dεx dz = K −3/2 + K −3/2 ρxy1 (z − z ) N dz 0 −3/2

σxy

p

dεy

dεx (G + H) +H dz dz

−3/2

dz

p p dεy dεx ρ1 (z − z ) (H + F) + H dz αx = K dz dz 0 p z p dεy dεx −3/2 αy = K ρ1 (z − z ) (G + H) + H dz dz dz 0 z p M dεx αxy = K −3/2 dz ρxy1 (z − z ) N dz 0 −3/2

(9.49b)

(9.49c)

z

(9.49a,b) may be further written as p p dεy dεx +H = (H + F) dζ dζ p p dεy dεx +H = (G + H) dζ dζ

(9.50)

σx − αx K −3/2 f σy − αy K −3/2 f

(9.51)

which may then be solved for p

M

(G + H)(σx − αx ) H(σy − αy ) dεx = − dζ K −3/2 f K −3/2 f p

M

dεy dζ

=

(H + F)(σy − αy ) H(σx − αx ) − K −3/2 f K −3/2 f

(9.52a) (9.52b)

Also, (9.49c) is rewritten as p

σxy − αxy M dεxy = N dζ K −3/2 f

(9.52c)

Therefore, in an anisotropic sheet, it takes a multiaxial stress state to produce a single plastic strain component. Equations (9.52) may be viewed as the ﬂow rule using the concept of the ﬂow theory of plasticity. It may be easily

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

467

shown that the plastic strain increment as given by (9.52) is normal to the yield surface to be discussed in the next paragraph. We note that, in the theory of Section 9.2.1, the plastic strain increment is necessarily pointing along the radial direction, emanating from the center of the yield surface, and it is not normal to the yield surface after the yield surface has suffered a distortion. Finally, plastic incompressibility is assumed so that p

p

p

dεx + dεy + dεz = 0

(9.53)

It was established in [4] that the deﬁnition of the intrinsic time determines the form of the yield function. For sheet metals, we now show that the proposed deﬁnition of intrinsic time leads to Hill’s 1948 quadratic yield criterion. The intrinsic time is deﬁned using the concept of equivalent plastic strain increment discussed in the appendix of [9], that is, dζ = d¯ε =

(G + H) p p [(H + F)dεx + Hdεy ]2 K3

2H p p p p [(H + F)dεx + Hdεy ][(G + H)dεy + Hdεx ] K3 1/2 (H + F) 2N M p 2 p p 2 + [(G + H)dεy + Hdεx ] + 3 dεxy N K3 K

−

(9.54)

Upon substitution of ﬂow rule (9.51) or (9.52), we obtain from (9.54)

σy − α y σx − α x 2 2H σx − αx − K −3/2 f K 3 K −3/2 f K −3/2 f (H + F) σy − αy 2 2H σxy − αxy 2 + 3 − 1 dζ 2 = 0 + K3 K −3/2 f K K −3/2 f

(G + H) K3

(9.55)

Thus, either dζ = 0 and the quantity in the bracket { } = 0, or dζ = 0 and the bracket { } = 0. The cases of dζ = 0 and dζ = 0 correspond to the elastic and plastic behavior, respectively. In the latter case, after simpliﬁcation, we obtain (G + H)(σx − αx )2 − 2H(σx − αx )(σy − αy ) + (H + F)(σy − αy )2 + 2N(σxy − αxy )2 = f 2

(9.56)

This is an extended version of Hill’s yield criterion [10]. The isotropic hardening is expressed by f and the kinematic hardening is expressed by αx , αy , and αxy . Coefﬁcients F, G, H, and N are determined from experiments that p p together with the plastic strain ratio Rα = dεy /dεz are discussed further in Chapter 10. The plastic strain ratio is related to the test of a sheet type tension

© 2005 by Chapman & Hall/CRC Press

468

Continuum Mechanics and Plasticity

specimen, where x is along the longitudinal direction of the specimen, y is the transverse direction, and z = z. Show that the ﬂow rule given by (9.52) obeys the normality rule and is normal to the yield surface given by (9.56).

EXAMPLE 9.1

Solution The yield function from (9.56) is 2φ = (G + H)(σx − αx )2 − 2H(σx − αx )(σy − αy ) + (H + F)(σy − αy )2 + N(σxy − αxy )2 + N(σyx − αyx )2 − f 2

(a)

Let us perform the following partial differentiation ∂φ = (G + H)(σx − αx ) − H(σy − αy ) ∂σx ∂φ = −H(σx − αx ) + (H + F)(σy − αy ) ∂σy

(b)

∂φ = N(σxy − αxy ) ∂σxy Comparing (b) with (9.52), we see that the two sets of equations differ only by a scalar multiple factor. Therefore, we may conclude that (9.52) satisﬁes the normality condition.

9.3

Endochronic Plasticity in the Finite Strain Range

In [11], Valanis considered internal variables qr (r = 1, 2, . . . , n) as quantities which transform as tensors with rotation of the material coordinate system, but remain invariant with rotation of the spatial system. In [12], these variables were regarded as quantities that transform as tensors with rotation of the spatial coordinate system, giving rise to a spatial formulation of the thermodynamics of internal variables. For tensors in the material coordinate system, care was taken to distinguish between the covariant, contravariant, and mixed components. This distinction gave rise to different constitutive equations depending on which components were chosen as independent variables. Valanis [13] further investigated the stress rate and the rate of evolution for the back stress, and recommended that the convected rates be used. He distinguished the convected rate for covariant stress from that for contravariant stress, and applied them to show that, by use of the convected rates, Prager’s linear kinematic-hardening rule did not lead to an oscillatory shear stress–strain curve under simple shearing. It is well known

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

469

that the shear stress–strain curve oscillates when the Jaumann rate is used (Section 7.6.3). Valanis [13] further mentioned that while the two convected rates have clear and distinct physical meanings, the Jaumann rate is the average of the aforementioned two rates and the physical meaning is obscure. The convected rates are further discussed in Chapter 11 in conjunction with the curvilinear coordinate system. While the use of a convected rate is most appropriate for stress and kinematic variables, the use of a convected rate for the back stress is questionable. The back stress is a way to represent anisotropy resulting from the change of material texture due to plastic deformation. While Dafalias [14] uses the concept of plastic spin to account for the change of material texture (see Section 7.6.2), he cautions against associating the plastic spin with the general kinematics of deformation. The concept of plastic spin has been introduced into the endochronic theory by Im and Atluri [15] and Wu et al. [5]. We follow [5] in the remaining part of this section. We ﬁrst discuss the concept of a corotational integral, which is useful in the ensuing discussion of endochronic theory for large strain.

9.3.1

Corotational Integrals

Suppose that a ﬂexible body moves in space. The triad of unit vectors of frame x¯ i that rotates with the body coincides with that of the reference frame xi at time zero. The two sets of coordinates are related by

[¯x] = [M]T [x]

(9.57)

where [M] is the matrix of an orthogonal tensor, such that [M][M]T = [I]. Then, the following transformation laws apply [¯g] = [M]T [g] ¯ = [M]T [T][M] [T]

[g] = [M][¯g] T ¯ [T] = [M][T][M]

(9.58)

where [g] is the matrix of a ﬁrst-rank tensor and [T] is the matrix of a ¯ refer to the x¯ i frame and we may write their second-rank tensor; [¯g] and [T] corotational derivatives as ∇

g = [˙g] − [][g],

∇

˙ − [][T] + [T][] T = [T]

(9.59)

where T ˙ [] = [M][M]

© 2005 by Chapman & Hall/CRC Press

(9.60)

470

Continuum Mechanics and Plasticity

and a dot over a tensor denotes its material derivative. It is easy to show that · ∇

˙¯ T = [M][M]T [T][M][M]T T = [M][T][M]

(9.61)

The expressions of (9.61) show that the corotational rate of T with respect to the reference frame xi is obtained by ﬁnding the material rate of T¯ with respect to frame x¯ i and then transporting the result back to the reference frame xi . It may be shown that the corotational rate is objective by considering a superposed rigid body rotation Q, such that [M ] = [Q][M]. Thus, ¯ = [QM]T [T ][QM] = [M]T [Q]T [T ][Q][M] = [M]T [T][M] [T]

(9.62)

The last expression of (9.62) is obtained from (9.58) and we conclude from (9.62) that [T ] = [Q][T][Q]T

(9.63)

Therefore, by using the ﬁrst expression of (9.61), we obtain

∇

T

∇

∇

˙ T T ¯ = [M ][T][M ] = [Q][M] [M] T [M] [M]T [Q]T = [Q] T [Q]T

(9.64) which shows that the corotational rate is objective. Let us now consider the integral {T} of the second-order objective tensor T [16,17], which is a function of t and t , that is, T = T(t, t ). Here, t is the current time and t is a dummy parameter of integration. Referring to the corotational frame x¯ i , the integral is deﬁned as: ¯ = {T}

t 0

¯ t )]dt = [T(t,

t 0

[M(t )]T [T(t, t )][M(t )]dt = [M(t)]T {T}[M(t)] (9.65)

with {T} = [M(t)]

t 0

[M(t )]T [T(t, t )][M(t )]dt [M(t)]T

(9.66)

The integral {T} is known as the corotational integral. Physically, the corotational integral ﬁrst transfers the tensor T to the x¯ i frame to obtain T¯ and, after integration in the x¯ i frame, it transports the result back to the xi frame. Note that T(t ) is a special case of T(t, t ).

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

471

Let us consider the expression of the back stress α, which will be used later. Let the expression of back stress α for small deformation be α=

z

0

µ(z − z )

dεp dz dz

(9.67)

where z is the intrinsic time. We now extend expression (9.67) to large deformation by use of (9.66). The integrand of (9.67) is a second-order tensor, which becomes tensor µ(z − z )D/˙z in the case of large deformation. Then α is the corotational integral {µ(z − z )D/˙z}. It follows from (9.66) that [α] = [M(z)]

z 0

[M(z )]T [D][M(z )] µ(z − z ) dz [M(z)]T z˙

(9.68)

On the other hand, by use of (9.61), we obtain the corotational rate of α as ∇

T ˙¯ α = [M][α][M]

(9.69)

We further determine α˙¯ as follows ˙¯ = [α]

d[α] ¯ d[α] ¯ dz d[α] ¯ = = z˙ dt dz dt dz

(9.70)

Note that the dot represents material differentiation. In the study of constitutive equations, α is not a function of xi and, therefore, the material differentiation is the same as the ordinary differentiation. From (9.58) and (9.68), we obtain [α] ¯ = [M]T [α][M] =

z 0

µ(z − z )

[M(z )]T [D][M(z )] dz z˙

(9.71)

The derivative of (9.71) with respect to z is [dα] ¯ [M(z)]T [D][M(z)] = µ(0) + dz z˙

z 0

dµ(z − z ) [M(z )]T [D][M(z )] dz z˙ dz (9.72)

By substituting (9.72) and (9.70) in (9.69), we obtain the corotational rate of α as z ∇

dµ(z − z ) [M(z )]T [D][M(z )] [D] T α˙ = z˙ µ(0) dz [M] + [M] dz z˙ z˙ 0 (9.73)

© 2005 by Chapman & Hall/CRC Press

472

Continuum Mechanics and Plasticity

EXAMPLE 9.2

Show that the corotational integral {T} is objective.

Solution We consider a superposed rigid-body rotation Q, such that [M ] = [Q][M]. With reference to the primed system, (9.65) is written as ¯ = {T}

0

t

¯ t )]dt = [T(t,

t 0

[M (t )]T [T (t, t )][M (t )]dt = [M (t)]T {T }[M (t)] (a)

which can be rewritten as {T } = [M (t)]

t 0

[M (t )]T [T (t, t )][M (t )]dt [M (t)]T

t = [Q(t)][M(t)] [M(t )]T [Q(t )]T [Q(t )][T(t, t )][Q(t )]T 0

× [Q(t )][M(t )]dt [M(t)]T [Q(t)]T = [Q(t)][M(t)]

t 0

[M(t )]T [T(t, t )][M(t )]dt [M(t)]T [Q(t)]T

= [Q(t)]{T}[Q(t)]T

(b)

Equation (b) shows that the corotational integral {T} is objective. EXAMPLE 9.3 ∇

Show that the corotational integration of the corotational

derivative T recovers the original tensor T, if T = T(t ), that is, T is not a function of t. Solution From (9.66) and using the ﬁrst equation of (9.61), the corotational integral ∇

of T is ∇ T = [M(t)]

0

= [M(t)]

t

t 0

∇

[M(t )]T T (t ) [M(t )]dt [M(t)]T

˙¯ )]dt [M(t)]T = [M(t)][T][M(t)] T ¯ [T(t = [T]

(a)

Equation (a) demonstrates that the corotational integral of a corotational rate of a tensor is the tensor itself. Therefore, the corotational integral is the inverse operation of the corotational derivative.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity EXAMPLE 9.4

473

Consider the integral for small deformation given by α=

z 0

µ(z − z )

dεp dz dz

(a)

In the case of µ(z) = µ0 e−λz , where µ0 and λ are constant parameters, the differentiation of (a) gives rise to α˙ = µ0 ε˙ p − λα˙z

(b)

In the case of µ(z) = µ1 e−λz + µ2 , where µ(0) = µ1 + µ2 , µ1 , µ2 , and λ are constant parameters, the differentiation of (a) gives rise to α˙ = µ(0)˙εp − λα˙z + λµ2 z˙ εp

(c)

Extend (a) to large deformation and determine the corotational rates. Solution

For the case of µ(z) = µ0 e−λz , dµ(z−z )/dz = −λµ0 e−λ(z−z ) , (9.73) becomes z T ∇

) [M(z )] [D][M(z )] −λ(z−z T α = µ(0)[D] + z˙ [M] (−λ)µ0 e dz [M] z˙ 0 = µ0 [D] − λ˙z[α]

(d)

Note that (d) is in the same form as (b). When µ(z) = µ1 e−λz + µ2 , then from (9.68) [α] = [M(z)]

z

0

µ1 e

+ [M(z)]

z 0

−λ(z−z ) [M(z

)]T [D][M(z )]

z˙

dz

[M(z)]T

[M(z )]T [D][M(z )] µ2 dz [M(z)]T z˙

= [α](1) + [α](2)

(e)

where (1)

[α] [α]

(2)

= [M(z)] = [M(z)]

© 2005 by Chapman & Hall/CRC Press

z 0 z 0

µ1 e

−λ(z−z ) [M(z

)]T [D][M(z )]

z˙

dz

[M(z )]T [D][M(z )] µ2 dz [M(z)]T z˙

[M(z)]T (f)

474

Continuum Mechanics and Plasticity

The integral on the right-hand side of (9.73) is

dµ(z − z ) [M(z )]T [D][M(z )] dz [M]T z˙ dz 0 z T −λ(z−z ) [M(z )] [D][M(z )] = −λ[M(z)] µ1 e dz [M(z)]T = −λ[α](1) z˙ 0 (g)

[M]

z

Substituting (g) into (9.73), we obtain ∇

α = µ(0)[D] − λ[α](1) z˙ = µ(0)[D] − λ[α]˙z + λ[α](2) z˙

(h)

The corotational derivative (h) is not quite of the same form as (c).

9.3.2

Endochronic Equations for Finite Plastic Deformation

In the small strain range, the endochronic constitutive equation is from (8.93) and (8.125) σ = σy

dεp + dz

z 0

dεp dz dz

(9.74)

dζ = f (z) dz

(9.75)

µ(z − z )

The intrinsic time is dζ 2 = dεp · dεp

with

The following yield function may be derived (σ − α) · (σ − α) = (σy, f (z))2

(9.76)

with the ﬂow rule given by dεp =

dz (σ − α) σy

(9.77)

where f (z) is the isotropic hardening function and α is the back stress given by α=

z 0

µ(z − z )

dεp dz dz

(9.78)

This set of equations will now be extended to the ﬁnite strain range by use of stress and strain measures for ﬁnite deformation, the concept of corotational derivative and corotational integral, and the concept of constitutive

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

475

spin (Section 7.6.2). To this end, (9.75) and (9.77) are written as ζ˙ 2 = Dp · Dp

(9.79)

1 (σ − α)˙z σy

(9.80)

Dp =

We extend (9.78) to large deformation by use of (9.66) and the resulting equation, (9.68), is α = M(z) ·

MT (z ) · Dp · M(z ) µ(z − z ) dz · MT (z) z˙

z

0

(9.81)

The integration in (9.81) is with respect to z , which is not t as in (9.66). The intrinsic time z is a monotonically increasing parameter and it does not change during elastic deformation or rigid-body rotation. In general, M(z) is not a unique function of z, because rotation may continue even when z is not changing. This multivalued association of M(z) to z does not invalidate the meaning of integral (9.81), as pointed out by Dafalias [17]. For simplicity in the subsequent calculations, we consider µ(z) = µ1 exp(−λz) + µ2

(9.82)

The corresponding corotational rate of α has been found in Example 9.5 to be ∇

α = (µ1 + µ2 )Dp − λα˙z + λα(2) z˙

(9.83)

where (2)

α

= µ2 M(z) ·

z 0

MT (z ) · Dp · M(z ) dz · MT (z) z˙

(9.84)

Equation (9.83) is the evolution equation of the back stress in terms of the plastic strain rate Dp , the back stress α, and the intrinsic time z. Note that (9.83) is in the incremental form, except for α(2) , which is represented by an integral in (9.84). It is shown in the next section that in solving the problem of a thin-walled tube under torsion, this integral may be integrated so that (9.83) becomes a truly incremental form. The plastic spin, from (7.100), may be written as Wp =

© 2005 by Chapman & Hall/CRC Press

C1 ζ˙ (α · σ − σ · α) (σy f (z))2

(9.85)

476

Continuum Mechanics and Plasticity

where C1 is dimensionless and is a scalar function of the isotropic invariants of σ and α. Using the second expression of (9.75) and the ﬂow rule (9.80), (9.85) becomes C1 f (z)˙z (α · σ − α2 + α2 − σ · α) (σy f (z))2 C1 (σ − α)˙z (α − σ )˙z = + ·α α· σy f (z) σy σy

Wp =

=

C1 (α · Dp σy f (z)

− Dp · α) = K(α · Dp − Dp · α)

with K =

C1 σy f (z) (9.86)

The above expression is the same as (7.101). Equation (9.86) together with (7.138) is substituted into (9.83) when the corotational rate is used in the calculation. 9.3.3

Application to a Rigid-Plastic Thin-Walled Tube Under Torsion

In the consideration of a thin-walled tube under torsion in the large strain range, the elastic strain is neglected, so that the condition of plastic incompressibility is represented by ε˙ r + ε˙ θ + ε˙ z = 0

(9.87)

where ε˙ r denotes the plastic strain-rate in the radial direction; ε˙ θ denotes the plastic strain-rate in the tangential direction; and ε˙ z denotes the plastic strainrate in the axial direction of the tube. The plastic shear strain 2η is related to the angle of twist per unit length ϕ by 2η = rϕ

(9.88)

in which r is the outer radius of the tube. The rate of deformation and spin tensors are expressed as

ε˙ r [Dp ] = 0 0

0 ε˙ θ η˙

0 η˙ , ε˙ z

0 [W ] = 0 0

0 0 −η˙

0 η˙ 0

(9.89)

The equations in (9.89) are now used to derive the explicit expressions for plastic spin and back stress. Let the back stress be symmetric so that

αrr [α] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 αθθ αθz

0 αθz αzz

(9.90)

Topics in Endochronic Plasticity

477

Then, since Dp and α are symmetric, we note that Dp ·α = (α·Dp )T . Therefore, α · Dp − Dp · α 0 0 0 0 (αθθ − αzz )η˙ + αθz (˙εz − ε˙ θ ) = 0 0 −(αθθ − αzz )η˙ − αθz (˙εz − ε˙ θ ) 0 (9.91) Equation (9.91) is substituted in (9.86) to calculate the plastic spin Wp . On the other hand, the constitutive spin ω is deﬁned in (7.97) as

0 ω = W − Wp = 0 0

0 0 ω

0 −ω 0

(9.92)

where ω = K[(αθθ − αzz )η˙ + αθz (˙εz − ε˙ θ )] − η˙

(9.93)

Since the tensor α is symmetric and the tensor ω is antisymmetric, we have α · ω = −(ω · α)T . Therefore, in order to ﬁnd explicit expressions for the corotational rate, we ﬁrst ﬁnd

0 ω · α − α · ω = 0 0

0 0 −2ωαθz −ω(αzz − αθθ ) 2ωαθz −ω(αzz − αθθ )

(9.94)

Using (9.59), the corotational derivative of α is ∇

α = α˙ − ω · α + α · ω

(9.95)

We then obtain the following expressions by combining (9.95) and (9.83) ∇

α˙ = ω · α − α · ω + α = (ω · α − α · ω) + (µ1 + µ2 )Dp − λα˙z + λα(2) z˙ (9.96) where, from (9.84), α(2) = µ2

z 0

Dp dz z˙

(9.97)

In the last expression, it has been assumed that the corotational axes are parallel to the reference axes, so that M = 1. This is indeed the case for the torsion problems under consideration. The deformation is homogeneous

© 2005 by Chapman & Hall/CRC Press

478

Continuum Mechanics and Plasticity

without rigid-body motion of the tube and the angle of twist per unit length is constant along the tube. In the numerical calculation, we can deﬁne a tensor κ as 0 0 0 κ = ω dt = 0 0 −κ (9.98) 0 κ 0 in which the following expression has been determined by use of (9.93) κ = ω dt = K[(αθθ − αzz )dη + αθz (dεz − dεθ )] − dη

(9.99)

Then, (9.96) reduces to dα = (κ · α − α · κ) + (µ1 + µ2 )Dp dt − λ α dz + λ α(2) dz

(9.100)

The equations derived in this section can be used to describe the response of a thin-walled tube subjected to various combined axial–torsion loading conditions. Two special cases are considered in the following paragraphs. 9.3.3.1 Torsion with axial prestress Denoting the axial prestress by σz = σc = constant, the stress tensor and the deviatoric stress tensor are −σ c 0 0 3 0 0 0 −σc 0 τ and [σ ] = [σ ] = 0 0 τ (9.101) 3 0 τ σc 2σc 0 τ 3 Note that the hoop stress σθ is zero due to symmetry. The ﬂow rule is, from (9.80), (9.89), (9.90), and (9.101), written as σc /3 + αrr dεr =− , dz σy

dεθ σc /3 + αθθ =− dz σy

dεz 2σc /3 − αzz = , dz σy

τ − αθz dη = dz σy

(9.102)

The intrinsic time is then given from (9.79) and (9.89) by ζ˙ 2 = ε˙ r2 + ε˙ θ2 + ε˙ z2 + 2η˙ 2 = z˙ 2 f 2 (z)

(9.103)

Therefore, η˙ 2 =

© 2005 by Chapman & Hall/CRC Press

1 2

z˙ 2 f 2 (z) − ε˙ r2 + ε˙ θ2 + ε˙ z2

(9.104)

Topics in Endochronic Plasticity

479

By use of (9.87), (9.104) reduces to

1 2 2 z˙ f (z) − 2 ε˙ z2 − ε˙ θ ε˙ r 2 1 2 2 dεz 2 dεθ dεr = z˙ f (z) − 2 − 2 dz dz dz

η˙ 2 =

(9.105)

Substituting (9.102) in (9.105), we then obtain 2 2 σ 1 2σ 1 σ c c c ±dη = dz f 2 (z) − − αzz − + αrr + αθθ 2 σy 3 3 3 (9.106) The “+” sign is for loading and “−” is for unloading. To perform the numerical calculation of dα by use of (9.100), α(2) must ﬁrst (2) be determined. To obtain αθz from (9.97), we use (9.89) to get (2)

αθz = µ2

z 0

p

Dθz dz = µ2 z˙

η(z) η(0)

dη = µ2 η

(9.107)

In the last expression, the limits of integration are η(0) = 0 and η(z) = η. Similarly, we obtain the following components for α(2) during loading (2) αrr = µ2 εr ,

(2)

αθθ = µ2 εθ ,

(2) αzz = µ2 εz

(9.108)

Therefore, from (9.98), (9.100), (9.107), and (9.108), we obtain the following equations dαrr = (µ1 + µ2 )dεr − λαrr dz + λµ2 εr dz dαθθ = −2αθz κ + (µ1 + µ2 )dεθ − λαθθ dz + λµ2 εθ dz dαzz = 2αθz κ + (µ1 + µ2 )dεz − λαzz dz + λµ2 εz dz

(9.109)

dαθz = (αθθ − αzz )κ + (µ1 + µ2 )dη − λαθz dz + λµ2 η dz with the initial conditions η(0) = 0, εi (0) = 0, and αij (0) = 0. Thus, in a stepby-step calculation, we can use α = α + dα, εz = εz + dεz ,

εr = εr + dεr , η = η + dη

εθ = εθ + dεθ , (9.110)

Finally, we note that for the case of free-end torsion, the ends of the specimen are totally unconstrained with σc = 0. Thus, the equations for free-end torsion may be obtained by setting σc = 0 in the equations of this subsection.

© 2005 by Chapman & Hall/CRC Press

480

Continuum Mechanics and Plasticity

9.3.3.2 Fixed-end torsion In the case of ﬁxed-end torsion, ε˙ z = 0. Assuming incompressibility, we ﬁnd from (9.87) that ε˙ θ = −˙εr = 0. Hence, (9.89) becomes 0 0 ε˙ r (9.111) [Dp ] = 0 −˙εr η˙ 0 η˙ 0 Note that this is different from the simple shear assumption where ε˙ θ = 0. The stress tensor and the deviatoric stress tensor are −σ 0 0 3 0 0 0 −σ τ [σ ] = 0 0 τ and [σ ] = 0 (9.112) 3 0 τ σ 2σ 0 τ 3 in which σ may vary. Again, we mention that the hoop stress is zero, which is different from the simple shear assumption that σθ = 0. The ﬂow rule, from (9.80), has the following component equations: σ/3 + αrr dεr =− , dz σy αzz

2σ = , 3

σ/3 + αθθ dεθ =− , dz σy

dη τ − αθz = dz σy

(9.113)

The ﬁrst two equations of (9.113) may be combined to yield dεr αθθ − αrr = dz 2σy

(9.114)

The intrinsic time is then, from (9.79) and (9.111), given by ζ˙ 2 = 2˙εr2 + 2η˙ 2 = z˙ 2 f 2 (z) Therefore,

η˙ 2 = z˙ 2

1 2 f (z) − 2

dεr dz

(9.115)

2 (9.116)

Then, by substituting (9.114) in (9.116), we obtain 2 dz αθθ − αrr 2 ±dη = 2f (z) − 2 σy The “+” sign is for loading and “−” is for unloading. © 2005 by Chapman & Hall/CRC Press

(9.117)

Topics in Endochronic Plasticity

481

We may also obtain the following components of α(2) by using the same procedure as that which leads to (9.107) and (9.108) (2)

αθz = µ2 η,

(2) αrr = µ2 ε r ,

(2)

αθθ = −µ2 εr ,

(2) αzz =0

(9.118)

Therefore, from (9.98) to (9.100) and (9.118), we obtain the following component equations dαrr = (µ1 + µ2 )dεr − λαrr dz + λµ2 εr dz dαθθ = −2αθz κ − (µ1 + µ2 )dεr − λαθθ dz − λµ2 εr dz dαzz = 2αθz κ − λαzz dz dαθz = (αθθ − αzz )κ + (µ1 + µ2 )dη − λαθz dz + λµ2 η dz

(9.119)

with the initial conditions η(0) = 0, εr (0) = 0, and αij (0) = 0. We again use (9.110) for a step-by-step calculation.

9.3.3.3 Comparison of theoretical and experimental results In this section, we compare the theoretical and experimental results initially presented in [5] and reprinted here with permission from Elsevier. There are seven material constants in this model: c, β, C1 , σy , µ1 , µ2 , and λ where c and β are used in the isotropic-hardening function f (z) and describe the rate and saturation value of isotropic hardening; C1 ﬁxes the magnitude of plastic spin; σ√ y is a material constant proportional to the initial yield stress in shear (σy = 2τy ); and µ1 , µ2 , and λ are used in the kernel function µ(z), which describes the evolution of back stress. These material constants are determined by ﬁtting the theory to the experimental stress–strain curve during loading. After they have been determined, the constitutive equations are applied to predict experimental results of specimens subjected to different loading conditions. Three different materials have been investigated, 70 : 30 brass, Ni-200, and Al-1100. All shear strains reported in the experimental results are for the outer surface of the tubular specimen. For the 70 : 30 brass material, the material constants have been determined to ﬁt the experimental data of Stout (reported in Im and Atluri [15]) for the case of simple torsion (Figure 9.1). The constants are c = 3.1, β = 15.4, C1 = 4.5, σy = 90 MPa, µ1 = 200 MPa, µ2 = 50 MPa, and λ = 7.2. These constants are then used in the equations for torsion with axial stress σc = 0 (equations in Section 9.3.3.1) to predict behavior of the same material for two different strain paths, that is, monotonic and cyclic free-end torsion. The strain range of the monotonic torsion is from 0 to 4, whereas the specimen under cyclic loading is strained from 0 to 1.7, unstrained back to 0, and then restrained to 2.0. The results found from this theory are compared with the experimental data of Swift [18]. Figure 9.2 shows the axial strain of both monotonic and cyclic free-end torsion. It is seen that the theory does predict the trend of variation for the axial strain during torsion. We note that experiments of Swift and Stout were conducted in different laboratories and material conditions, and © 2005 by Chapman & Hall/CRC Press

482

Continuum Mechanics and Plasticity

Shear stress (MPa)

400

Experiment Theory

300

200

100

0 1

0

2 3 Shear Strain

4

5

FIGURE 9.1 Shear stress–strain curve of 70 : 30 brass (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

12

Monotonic loading Experiment Theory

Shear Stress (%)

10

Cyclic loading Experiment Theory

8 6 4 2 0 –1

0

1

2 Shear Strain

3

4

5

FIGURE 9.2 Axial strain versus shear strain for 70 : 30 brass (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

the agreement demonstrated here is therefore considered as very satisfactory. The effect of C1 is investigated and shown in Figure 9.3 for 70 : 30 brass. This ﬁgure shows the dependence of the axial strain on C1 in the case of monotonic free-end torsion. It is seen that a suitable C1 can be determined to achieve a good agreement with the experimental results.

© 2005 by Chapman & Hall/CRC Press

Axial Strain

Topics in Endochronic Plasticity

483 C1 = 0

35 30 25 20 15 10 5

C1 = 1 C1 = 2 C1 = 5 C1 = 10 C1 = 50 1

2 3 Shear Strain

4

FIGURE 9.3 Effect of parameter C1 of plastic spin on the axial strain during torsion (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

100 90 80

Shear Stress (MPa)

70 60 50 40 30 20 10 0 0

0.2

0.4

0.6

0.8 1 Shear Strain

1.2

1.4

1.6

1.8

FIGURE 9.4 Shear stress–strain curve of Ni-200 with 0.01 MPa axial prestress (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

The experimental data for Ni-200 are taken from Hart and Chang [19]. The material constants have been determined by ﬁtting the shear stress– strain curve (Figure 9.4) which was determined from torsion with a 0.01 MPa prestress. The constants have been determined to be c = 14.2, β = 5.5, C1 = 9, σy = 40 MPa, µ1 = 45 MPa, µ2 = 40 MPa, and λ = 9.5. Using these constants and the constitutive equations of Section 9.3.3.1, we have predicted the axial

© 2005 by Chapman & Hall/CRC Press

484

Continuum Mechanics and Plasticity 0.7 Prestress: Experiment

0.6 0.5

Theory

Axial Strain (%)

0.4

1.48 MPa 0.01 MPa –1.52 MPa

A

A 1.48 MPa B 0.01 MPa C –1.52 MPa B

0.3 0.2 C

0.1 0 –0.1 –0.2 0

0.05

0.1

0.15 0.2 0.25 Shear Strain

0.3

0.35

0.4

FIGURE 9.5 Axial strain for Ni-200 during torsion with axial prestresses (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

strain associated with torsion with prestresses of 1.48, 0.01, and −1.52 MPa. The results, shown in Figure 9.5, are quite satisfactory. Figure 9.6 shows the experimental shear stress–strain curve under simple shear condition (ﬁxed-end torsion), obtained by White et al. [20] for Al-1100 material. The theoretical result of the present theory is also shown. The material constants are c = 2.14, β = 4.5, C1 = 4.5, σy = 55 MPa, µ1 = 1.8 MPa, µ2 = 0.15 MPa, and λ = 1.64. Wu and Xu [21] also obtained a shear stress– strain curve for Al-1100, but in a smaller deformation range (12% strain). The curve agrees with the one shown in Figure 9.6. Using these constants and the constitutive equations of Section 9.3.3.1, we predicted the axial strain in the case of torsion with prestresses of −6.9 and −20.7 MPa. The results found from this theory (the solid and dashed curves) are compared with the experimental data of Wu and Xu [21] and shown in Figure 9.7. Figure 9.8 shows the prediction (the solid and dashed curves) of the hoop and axial strains, respectively, for the free-end torsion condition (i.e., with σc = 0). The experimental data of Bailey et al. [22] are also shown in the ﬁgure. Even though the theory agrees well with experiment in terms of the axial strain, there are discrepancies in the hoop strain at large shear strain level. These discrepancies may be explained by taking a closer look at the specimens and the procedure used in the experiments of Bailey et al. [22]. The specimens used

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity 250

485

Theory Experiment

Shear stress (MPa)

200

150

100

50

0 0

0.05

0.1

0.15

0.2 0.25 0.3 Shear Strain

0.35

0.4

FIGURE 9.6 Shear stress–strain curve of Al-1100 (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

0

–0.2

Axial Stress (%)

–0.4

–0.6

–0.8

–1

–1.2

Prestress = –6.9 MPa Prestress = –20.7 MPa

–1.4 0

0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09

0.1

Shear Strain FIGURE 9.7 Axial strain for Al-1100 during torsion with compressive axial prestresses (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

486

Continuum Mechanics and Plasticity 10

Axial strain Hoop strain

8 6 4

Strain (%)

2 0 –2 –4 –6 –8 –10 0

1

2

3

4 5 6 Shear Strain

7

8

9

10

FIGURE 9.8 Hoop and axial strains under free-end torsion (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

by them had a very short gauge length of 3.2 mm (0.125 in.) compared with a radius of 19 mm (0.75 in.). The radius of the relatively rigid ends of the specimen did not change, which in turn restricted the development of hoop strain at large shear strain level. Another possible restriction on the hoop strain is due to a plug and sleeve inserted into the specimens to prevent buckling at large strain level. The authors thought that there was sufﬁcient clearance to allow for any reduction in diameter during test. However, we believe that there was contact between the specimens and the plug at large shear strain level and, therefore, the reduction in diameter was restricted. If there were no contact, then the plug would not have been needed in the experiment. We believe that these are the reasons causing the experimental hoop strain to be on the low side compared with the theoretical result. Wu et al. [23] conducted the same experiments using extruded high purity aluminum with specimens of a much longer gauge length (82.6 mm or 3.25 in.) and without the plug. The outer radius of the specimens was 19 mm (0.75 in.). The results are shown in Figure 9.9. It is seen that these curves have the same trends as those of the theoretical curves shown in Figure 9.8, that is, the hoop and axial strains at large shear strain level have almost the same magnitude, whereas the results of Bailey et al. [22] show that the hoop strain does not increase much with the axial strain at large shear strain level. In some published writings such as Canova et al. [24], the rate of hoop strain is assumed to be equal to the rate of radial strain, ε˙ θ = ε˙ r , for a thin-walled

© 2005 by Chapman & Hall/CRC Press

Axial and Hoop Strain (%)

Topics in Endochronic Plasticity

487

6 al S Axi

4 2

–2 –4

train

Shear Strain (%) 25

50

75 100 125 150 175 Hoo p Str ain

–6

FIGURE 9.9 Experimental hoop and axial strains under free-end torsion (From Wu, H.C. et al, Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

tube under tension–torsion loading condition. This assumption is good only for the axial loading condition. Taylor and Quinney [25] showed that the hoop strain is not equal to the radial strain under combined tension–torsion loading. In this calculation, we have found that the rate of radial strain is almost zero, that is, the wall thickness changes very little. And, from (9.87), the magnitude of the hoop strain is nearly the same as that of the axial strain, in agreement with the experimental observation. We mention that the analysis of Lowe and Lipkin [26] and Qian and Wu [27], by use of polycrystal plasticity, also leads to the same trends as predicted by our theory for the axial and hoop strains.

9.4

An Endochronic Theory for Porous and Granular Materials

Porous-granular (PG) material is a class of material that includes geotechnical materials (concretes, rocks, soils, ice, etc.), porous metals made out of metal powders by sintering, and ceramics. The response of PG materials to loading generally consists of four parts, that is, the hydrostatic response, the deviatoric response, the shear-enhanced volumetric response, and the hydrostatic pressureenhanced shear response. A signiﬁcant characteristic of this class of materials is the existence of voids (or cracks) within the material. The pores collapse and close or grow under loading–unloading conditions, and material is either consolidated or damaged. This process is irreversible (plastic deformation and damage) and upon removal of the load a permanent change in the volume of the specimen is observed. Thus, plastic volumetric strain occurs when PG materials are subjected to hydrostatic pressure. Figure 9.10 shows a schematic volumetric stress–strain curve with both the initial and the ﬁnal slopes equal to the elastic bulk modulus K0 . The deviatoric stress–strain response for this class of materials is similar to that observed for metallic materials. A phenomenon similar to yielding occurs as the deviatoric stress–strain curve bends toward the strain axis.

© 2005 by Chapman & Hall/CRC Press

Continuum Mechanics and Plasticity

Hydrostatic Stress

488

Volumetric Strain FIGURE 9.10 Schematic volumetric stress–strain curve for porous-granular materials (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

0 < th

Volumetric Strain

0

Shear Strain

0 < th 0

Shear Strain 0 > th

0

Shear Strain

FIGURE 9.11 Shear-enhanced volumetric strain (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

A special property of PG materials is that during the application of deviatoric stress, a specimen exhibits a volumetric change that can either be a contraction or dilation depending on the state of hydrostatic stress σ 0 as compared with a threshold stress σ th within the specimen. This coupled behavior between volumetric and deviatoric responses is generally referred to as the shear-enhanced volumetric strain or densiﬁcation in soil mechanics. Figure 9.11 illustrates this behavior. Another coupled behavior is the hydrostatic pressure-enhanced shear deformation, which is sometimes referred to as the shear travel. In the last effect, additional deviatoric deformation occurs as the hydrostatic stress increases, while keeping the deviatoric stress constant. Figure 9.12 shows that along stress-paths BC, DE, and FG, on which the deviatoric stress is kept constant, shear travel occurs as is seen by the increase

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

489 G G F

Hydrostatic Stress

E

C

F

E

D z

C

B

D

Hydrostatic Axis

A A O

B

O

2x,y

Deviatoric Strain

FIGURE 9.12 The shear travel effect (From Wu, H.C. and Aboutorabi, M.R., Int. J. Plasticity, 4, 163, 1988. With permission from Elsevier).

in the deviatoric strain for each of the path segment. A threshold deviatoric stress may be deﬁned above which the shear travel strain is positive and below which it is negative. The hydrostatic and deviatoric responses may be viewed as the primary behavior while the coupled responses are secondary. In a theoretical treatment, the degree of importance of each response is therefore different. The hydrostatic and deviatoric responses should be the main part of a constitutive equation and they are directly related to both yield surface and ﬂow rule if such concepts are used in the formulation. However, there may indeed be cases in which no such concepts are used. In such cases, the hydrostatic and deviatoric responses should still be the main part of a constitutive equation. The coupled effects are secondary and can be accounted for by the ﬂow rule or by the evolution equation of a parameter. They also inﬂuence the shape of yield surfaces. In the case of soils, the most common test for the study of their mechanical behavior has traditionally been the conventional constant conﬁning pressure triaxial test (simply known as the conventional triaxial compression, CTC). In such a test, a cylindrical specimen is prepared in a ﬂexible membrane of a material such as polyurethane, and is placed in a chamber that can be pressurized, usually by ﬁlling it with water. An all-around constant conﬁning pressure is applied. Then, a loading ram can be used to apply an axial load along the long axis of the cylinder. In this test, the mean stress increases with the axial load and the observed stress–strain behavior is a combination of hydrostatic–deviatoric behavior. This test is denoted by CTC in Figure 9.13 and the stress path for this test is making an angle with HC (the hydrostatic compression). The stresses in this ﬁgure are principal stresses. σz is the axial stress of the cylindrical specimen. Unconﬁned compression tests (UC) and conﬁned compression tests (CC) have been used to test materials such as concretes, rocks, and ice. Cylindrical specimens are tested in the axial

© 2005 by Chapman & Hall/CRC Press

490

Continuum Mechanics and Plasticity z TC

UC

CTC

HC

CC TE 2 x,y

FIGURE 9.13 Illustration of various tests in the stress space.

direction either with free lateral surface (UC) or conﬁnement in a rigid cell (CC). The lateral stress builds up with increasing axial stress in the CC test. Both tests involve the mean stress and the deviatoric stress. The aforementioned traditional tests are not designed to separate the hydrostatic behavior from the deviatoric behavior. Since both behaviors are of primary importance in the characterization of PG materials, the true triaxial test has been developed to test the hydrostatic and deviatoric behaviors separately. The true triaxial device permits application of three independent (principal) stresses on a cubical specimen. The application of the stresses can be such that any path of loading in the three-dimensional stress space can be followed. Some of the paths are shown in Figure 9.13. The HC path corresponds to the application of an all-around hydrostatic pressure in isotropic consolidation. TC stands for triaxial compression and TE stands for triaxial extension. In the latter two tests, the deviatoric stress is applied under the condition of constant hydrostatic pressure, enabling us to concentrate on the deviatoric stress–strain response. Finally, we mention that direct shear testing and torsion of a solid shaft have also been conducted by researchers to characterize material behavior in shear. In this section, a version of endochronic theory of plasticity is presented that accounts for all the aforementioned responses. This theory has been derived based on the work of Wu and Aboutorabi [28] and Wu [29]. It is presented here with permission from Elsevier. We present the theory ﬁrst and its applications to concretes, sand, and porous aluminum are discussed.

9.4.1

The Endochronic Equations

The theory as derived in [28] has four elements corresponding to those previously mentioned. It has been modiﬁed in [29] so that the strain-rate sensitivity may be accounted for. The stress–strain curve is decomposed into volumetric and deviatoric stress–strain curves. The decomposition gives insight into

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

491

material behavior and is of special importance due to the signiﬁcant role played by the plastic volumetric deformation. This theory uses the Gibbs formulation described in Section 8.3.4. The Gibbs free energy is a function of stress σ and two groups of internal variables, γ and π. There are h number of γ’s related to the volumetric deformation and s number of π’s related to the deviatoric deformation. The reason for using the Gibbs formulation is that the hydrostatic and deviatoric stresses may be independently varied, which is a requirement for the derivation of the set of equations to be discussed in this chapter. This requirement is difﬁcult to satisfy in the Helmholtz formulation, since in that case the strain, ε is used as an independent variable and it is difﬁcult to independently vary the volumetric and the deviatoric strains for the PG materials. A hydrostatic intrinsic time zH is deﬁned to register the history of volumetric deformation, and a deviatoric intrinsic time zD is used to register the history of deviatoric deformation. In the Gibbs formulation, strain εij is given by εij = −

∂ ∂σij

(9.120)

and the evolution equations for γijh and πijs are given by h dγkm =0 dzH

(h not summed)

s dπkm ∂ s + N =0 ijkm ∂πijs dzD

(s not summed)

∂ ∂γijh

h + Mijkm

(9.121)

h and M s are positive semideﬁnite fourth-order isotropic constant where Mijkl ijkl tensors. These linear evolution equations are chosen for mathematical simplicity and they can be nonlinear if. However, they are shown to be adequate for the class of materials under consideration. These evolution equations are related to the rate of entropy production within the material. By expanding the Gibbs free energy in series and using only the quadratic and linear terms, the expression for may be substituted into (9.120) to (9.121). Each resulting equation can then be divided into volumetric and deviatoric parts. By doing so, it may be found that the volumetric strain εkk is the sum of the H , and densiﬁcation strain, ε S . The deviatoric strain e is hydrostatic strain, εkk ij kk the sum of strain due to deviatoric loading, eijS , and strain developed due to the coupling with the hydrostatic loading, eijH . The internal variables are divided into two parts as h γijh = 13 δij γkk + gijh ,

© 2005 by Chapman & Hall/CRC Press

s πijs = 13 δij πkk + pijs

(9.122)

492

Continuum Mechanics and Plasticity

where gijh is the deviatoric part of γijh , pijs is the deviatoric part of πijs , and δij is the Kronecker delta. The intrinsic times ζH and ζD are deﬁned by dζH = kH θ˙kk |dθkk |

and

˙ 2 dQij dQij dζD2 = kD (Q)

(9.123)

where the volumetric strain-like increment dθkk is deﬁned as H dθkk = dεkk − k1

dσkk 3K0

(9.124)

and the deviatoric strain-like tensor dQij is deﬁned as dQij =

deijS

− k2

dσij

(9.125)

2µ0

where σ = σkk /3 = mean pressure, σij = deviatoric stress; k1 and k2 are constants between 0 and 1. In the limiting case that k1 = k2 = 1, θkk reduces to the usual deﬁnition of volumetric plastic strain and Qij reduces to the deviatoric plastic strain. K0 is the bulk modulus and µ0 is the shear modulus. ˙ are the strain-rate sensitivity functions (see The functions kH (θ˙kk ) and kD (Q) Section 8.4.6), which enable the description of the strain-rate sensitive stress– strain behavior in the volumetric and deviatoric responses, respectively. 1/2 . ˙ ˙ ˙ where Q ˙ = (1Q These are functions of the strain-rates θ˙kk and Q, 2 ij Qij F) The following expressions may be used

θ˙kk kH (θ˙kk ) = 1 − kh log ˙θkk0

,

˙ = 1 − kd log kD (Q)

˙ Q ˙ Q0

(9.126)

˙ 0 are reference strain rates usually where kh and kd are constants; θ˙kk0 and Q taken as the lowest strain rates of the test series. Then, the following deﬁnes the governing equations for each component of strain: Volumetric: H = 3A0 σkk + 3 εkk

h Bh0 γkk

h

dγ h M0h kk dzH

h + Eh0 γkk − Bh0 σkk = 0

dζH = h(ζH ) dzH

© 2005 by Chapman & Hall/CRC Press

for all h (no sum on h)

(9.127)

Topics in Endochronic Plasticity

493

Deviatoric: eijS = A2 σij +

C2s pijs

s

dpijs N2s dzD

+ F2s pijs − C2s σij = 0

for all s (no sum on s)

(9.128)

dζD = f (ζD , σ 0 ) dzD Shear-enhanced volumetric strain: S = εkk

s s s C0 πkk

dπ s

s − Cs (σ − ξ ) = 0, N0s dzkk + F0s πkk 0 kk D

dπ s

s − Cs σ = 0, N0s dzkk + F0s πkk 0 kk D

s=1

(9.129)

s = 1

Pressure-enhanced shear strain: eijH =

h h h B2 gij

dgh

M2h dz ij + Eh2 gijh − Bh2 (σij − Dij ) = 0, H

dgh

M2h dz ij + Eh2 gijh − Bh2 σij = 0, H

h=1

(9.130)

h = 1

In the above equations, f (ζD , σ 0 ) = the deviatoric-hardening function, σ 0 = conﬁning hydrostatic stress at initial shear loading, A0 , A2 , Bh0 , Bh2 , C0s , C2s , Eh0 , Eh2 , F0s , F2s , M0h , M2h , N0s , N2s = parameters of the theory (for engineering application, they can be combined and the number of material constants reduced), ξ = threshold mean conﬁning pressure, Dij = threshold deviatoric stress. The equations for hydrostatic and deviatoric responses are now further investigated. These equations can be written in a form such that, in the limiting case of k1 = k2 = 1, yield conditions can exist with respect to both the hydrostatic and deviatoric stresses. This case also enables a geometric representation of the model in the stress space, so that the physical meaning of the model may be visualized. The geometric representation is further explained. The values of k1 and k2 do not have to be one. A value of 0.95 has been found to facilitate numerical computation. In this case, the constitutive equations are continuous and there is the advantage of not having to deal with the yield conditions in the numerical calculation. This aspect is indeed a very important strength of the present approach. In this way, even though yield stress is deﬁned in the theory, it can be circumvented during computation by assuming k1 not equal to one. In this approach, the results will be closely related to

© 2005 by Chapman & Hall/CRC Press

494

Continuum Mechanics and Plasticity

those obtained from the case of k1 = k2 = 1, where the yield conditions are used. The equations for hydrostatic and deviatoric responses are considered further in the following subsections.

9.4.1.1 The hydrostatic response H and the linear evolution for internal The volumetric strain increment dεkk h are from (9.127) given by variable γkk H = 3A0 dσkk + 3 dεkk

h dγkk Bh Eh h = 0h σkk − 0h γkk dzH M0 M0

h Bh0 dγkk ,

h

(9.131)

In order to account for strain hardening, the intrinsic time zH is scaled by dζH = h(θkk , ζH ) dzH

(9.132)

where the function h represents isotropic hardening and the increment of volumetric intrinsic time dζH > 0 is deﬁned in terms of plastic strain as in (9.123). The form of the hardening function is h(θkk ) =

C − (C − θm )e−µθkk θm − θkk

(9.133)

This form accounts for the experimentally observed fact that as material compacts, its ability to undergo plastic volumetric strains diminishes and eventually an elastic response is observed with a modulus equal to the initial bulk modulus. Thus, a maximum plastic volumetric strain of θm may be achieved. The material constants C and µ control the extent and rate of isotropic hardening. The values of these constants may be adjusted to ﬁt the volumetric stress–strain curves of various PG materials, including soil. By the substitution of (9.123), (9.124), (9.132), and the second equation of (9.131) into the ﬁrst equation of (9.131), the following equations may be found H dεkk [1 ± X] =

dσkk [1 ± k1 X] 3K0

(9.134)

where X=

Xh

h

© 2005 by Chapman & Hall/CRC Press

with X h =

Bh0 hM0h

h = Bh0 σkk − Eh0 γkk

(9.135)

Topics in Endochronic Plasticity

495

h = 0. Hence, the constant A may be Note that k1 = 1 and initially σkk = γkk 0 identiﬁed, that is, A0 = 1/9K0 and when h → ∞, (9.134) yields

dσkk 1 · 3 K0

H = dεkk

(9.136)

Equation (9.136) indicates a linear stress–strain response with a slope equal to the initial bulk modulus at large volumetric strain. When loading reverts to unloading the only change in the equations takes place in (9.134), where the negative sign in the brackets changes to positive. Note that in this investigaH and the current tion, tensile stress is considered to be positive. Knowing dεkk h values of zH , σkk and γkk , (9.134) may be used to calculate dσkk . (9.123), (9.124), and (9.132) can then be used to determine dθkk and dzH , and (9.131) leads to h . Therefore, z , σ , and γ h can be updated. This step-by-step procedure dγkk H kk kk is used to calculate the volumetric stress–strain curve. For the case of k1 = 1, it is shown now that the previous equations can describe a physical situation when the material experiences a combined isotropic–kinematic hardening in the volumetric behavior. Both tensile (further limited by fracture) and compressive hydrostatic stresses are included in this discussion and it is shown that the combined isotropic–kinematic hardening arises naturally in the volumetric response of the endochronic formulation. To this end, the ﬁrst equation of (9.131) is solved for dσkk and the result substituted into (9.124) to obtain H + 3k1 dθkk = (1 − k1 )dεkk

Bh Bh 0 0

h

=

H ϕkk

M0h

σkk −

Bh Eh 0 0

h

M0h

h dzH γkk

H + ψkk dzH

(9.137)

where H H = (1 − k1 )dεkk ϕkk Bh Bh Bh E h H 0 0 0 0 h ψkk = 3k1 σ − γ h kk h kk M M 0 0 h h

(9.138)

But, from (9.123) and (9.132), H H h dzH = dζH = ±kH dθkk = ±kH (ϕkk + ψkk dzH )

(9.139)

or H ∓ βkk

© 2005 by Chapman & Hall/CRC Press

h kH

H dzH + ϕkk =0

(9.140)

496

Continuum Mechanics and Plasticity

H = 0. Thus, When k1 = 1, ϕkk

H ψkk ∓

h kH

dzH = 0

(9.141)

Since during plastic deformation, dzH = 0, then, H =± ψkk

h kH

(9.142)

By substituting (9.138) into (9.142), it is found that y

H σkk − αkk

σ = ± kk h kH

(9.143)

where y σkk

= 3

Bh Bh

−1

0 0 M0h

h

y

H αkk = 3σkk

and

Bh Eh 0 0

h

M0h

h γkk

(9.144)

This expression may be viewed as a yield criterion for hydrostatic stress with y H denoting the kinematic σkk h/kH denoting the isotropic hardening and αkk y hardening. Note that in the isotropic hardening, σkk is the initial quasistatic yield stress, which when divided by kH becomes the dynamic yield stress. h is the isotropic-hardening function. The ﬂow rule is given from (9.137) by dzH

H dzH = dθkk = ψkk

9.4.1.2

y

σkk

H (σkk − αkk )

(9.145)

The deviatoric response

In the deviatoric response, from (9.128), the equations are deijS

=

A2 dσij

+

dpijs

C2s dpijs ,

dzD

s

=

C2s F2s s σ − p N2s ij N2s ij

(9.146)

Note that the evolution of pijs is deﬁned with respect to the deviatoric intrinsic time zD . For the ﬁrst increment of loading from the virgin state, since σij = pijs = 0, (9.146) yields

deijS dσij

© 2005 by Chapman & Hall/CRC Press

= A2 0

(9.147)

Topics in Endochronic Plasticity

497

Therefore, A2 is identiﬁed as the inverse of the initial slope 2µ0 of the deviatoric stress–strain curve. Thus, A2 = 21 µ0 . The deviatoric intrinsic time increment dζD is deﬁned as in (9.123) and is related to zD through the hardening function f (zD ) deﬁned by (9.128). It will be shown subsequently that function f represents isotropic hardening in the deviatoric behavior. Solving the ﬁrst equation of (9.146) for dσij and substituting the result together with the second equation of (9.146) into (9.125) yields dQij = ϕijD + ψijD dzD

(9.148)

ϕijD = (1 − k2 )deijS Cs F2s s 2 ψijD = k2 C2s σ − p N2s ij N2s ij s

(9.149)

where

Then, by substituting the third equation of (9.128) and (9.148) into (9.123), the following quadratic equation is obtained 2 P dzD + W dzD + R = 0

(9.150)

where P = ψijD ψijD −

f kD

2 ,

W = 2ϕijD ψijD ,

R = ϕijD ϕijD

(9.151)

Therefore, P, W , and R are functions that are deﬁned in terms of the constants of the model and increments of input variables. When (9.150) is solved for dzD , the second equation of (9.146) can be used to obtain dpijs . By substitution, the deviatoric stress increment dσij can then be found from the ﬁrst equation of (9.146). In the case of k2 = 1, (9.149) and (9.151) give ϕijD = R = W = 0. Thus, (9.150) 2 = 0. Since dz = 0 when there is plastic deformation, is reduced to P dzD D P must be zero. Hence, the ﬁrst equation of (9.151) leads to (σij

− αijD )(σij

− αijD )

=

σy f

2 (9.152)

kD

where σy

=

Cs Cs s

© 2005 by Chapman & Hall/CRC Press

2 2 N2s

−1 ,

αijD = σy

Cs F s

2 2 s pij

s

N2s

(9.153)

498

Continuum Mechanics and Plasticity

This is the Mises yield criterion with combined isotropic–kinematic hardening, in which σy f /kD describes the isotropic hardening and αijD the kinematic hardening in the deviatoric behavior. Note that in the isotropic hardening, σy is the quasistatic deviatoric yield stress, which when divided by kD becomes the dynamic yield stress and f is the isotropic-hardening function. From (9.148), the plastic strain increment is now given by p

deij = ψijD dzD =

dzD σij − αijD σy

(9.154)

which is normal to the deviatoric yield surface. It has thus been shown that in the case of k1 = k2 = 1, the present endochronic theory is equivalent to a ﬂow theory of plasticity, which obeys the Mises yield criterion with combined isotropic–kinematic hardening, both in the hydrostatic and deviatoric responses. 9.4.1.3 Geometric representation of the model There is a simple geometrical representation of the proposed model for the case of k1 = k2 = 1, in which two yield criteria are deﬁned, one for volumetric behavior and the other for deviatoric behavior. The material constants of the model depend on the initial density of the material, and these constants are then used to describe subsequent material behavior. The two yield criteria exist in a space plotting the hydrostatic stress σkk /3 against the equivalent stress σeq , which is deﬁned as the square root of the second invariant of the deviatoric stress tensor (see Figure 9.14). The volumetric yield criterion is represented by two vertical yield lines and the deviatoric yield criterion by two horizontal yield lines. These yield lines are not necessarily straight due to the cross effects between the hydrostatic and deviatoric responses. These are shown by the thin curves in Figure 9.14. The distance eq Vol. Elastic Line

Vol. Yield Line

Deviatoric Yield Line 0

Vol. Yield Line

kk/3

Deviatoric Yield Line

FIGURE 9.14 Geometric representation of the model (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

499

between the yield lines can expand, resulting in isotropic hardening. The two yield lines as a set can also move, resembling the kinematic hardening. According to this model, combined isotropic–kinematic hardening takes place in both the volumetric and deviatoric responses. A volumetric elastic line may be established in the hydrostatic compression region indicating a limit beyond which the volumetric response is elastic again. This phenomenon corresponds with the bending upward of the volumetric stress–strain curve at large strain level, where the modulus is elastic. According to this model, the volumetric and deviatoric yield limits are individually imposed. The model allows for the situation that yielding has already occurred volumetrically but not yet occurred deviatorically. This is a situation that is frequently observed in sands, which have a very low volumetric yield limit. Thus, the deviatoric response in this case would initially be elastic and then plastic when the deviatoric yield limit is reached. In the case of sand, the volumetric yield lines are collapsed into a line passing through the origin as shown in Figure 9.15. In this ﬁgure, compressive stress is considered positive as is the usual practice of soil mechanics. The failure lines (FL) are shown together with lines showing the initial yield lines and the subsequent yield lines obtained by isotropic and kinematic hardening, respectively. The idea of volumetric compaction yield surface and shear yield surface and ! of representing them as horizontal and vertical straight lines in the J1 versus J2 space was brieﬂy mentioned by Johnson and Green [30]. This idea is similar to the present model and is described by the endochronic constitutive equations of this section.

eq FL

Subsequent YL Deviatoric initial YL

kk/3

0

Volumetric YL

Kinematic hardening Initial YL Isotropic hardening FL

FIGURE 9.15 Yield lines for sand (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

© 2005 by Chapman & Hall/CRC Press

500

Continuum Mechanics and Plasticity deijh

eq

dQij

dQij

TC

s dkk

dkk

s dkk

CT or C PL

Deviatoric YL

dkk

0

HC

kk/3

Volumetric YL

FIGURE 9.16 Plastic strain increments of the model (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

The volumetric plastic strain increment dθkk is given by (9.145) and the deviatoric plastic strain increment dQij is given by (9.154), which is normal to the deviatoric yield surface. These equations resemble the ﬂow rule of a ﬂow theory of plasticity. However, additional plastic strain increments S and deH need to be considered in this model. These increments are due dεkk ij to coupled effects as discussed earlier and the occurrence of the increments depends on the stress path. Figure 9.16 shows the plastic strain increments associated with various stress paths in a true triaxial test. A hydrostatic compression test (HC) will give rise to dθkk only; a TC test will give rise to dQij S ; and a CTC test or a proportional loading test (PL) will lead to all and dεkk S , and deH . It is difﬁcult to compare the four increments, that is, dθkk , dQij , dεkk ij present plastic strain increments with the associative or nonassociative ﬂow rules of the classical theory. In that theory, the direction of the total plastic strain increment is investigated with respect to a plastic potential in the stress space, and combines both the deviatoric and hydrostatic behaviors. Whether the ﬂow rule is associative or nonassociative is still a point of debate. In the present model, no such complication is involved, however.

9.4.2

Application to Concrete

The endochronic theory of the previous section has been applied in [28] to investigate the experimental results of concrete reported by Scavuzzo et al. [31]. Cubical specimens were tested under a true triaxial test. In such a test, σx , σy , σz are principal stresses and εx , εy , εz are principal strains.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

501

The material is not strain-rate sensitive and the strain-rate sensitivity functions are kH = kD = 1. For the isotropic-hardening functions, (9.133) is used for h and the form for f is chosen as f (zD ) = Cp − (Cp − 1)e−µzD

(9.155)

where Cp and µ are constants. Equations of Sections 9.4.1.1 and 9.4.1.2 are used to describe the hydrostatic and deviatoric behaviors. In the consideration of shear-enhanced volumetric strain, we use two internal variables, and (9.129) becomes S 1 2 εkk = C01 πkk + C02 πkk 1 dπkk C1 = 0 (σkk − ξ ), dzD N

2 dπkk C2 F2 2 = 0 σkk − 0 πkk dzD N N

(9.156)

All deviatoric constants associated with the internal variable π 1 are assumed to be zero. The above equations may be combined to yield S dεkk S = I 1 (σkk − ξ ) − χ 2 εkk + I1χ 2 dzD

zD 0

(σkk − ξ ) dzD + I 2 σkk + χ 2 π0 (9.157)

where I1 =

C01 C01 , N

I2 =

C02 C02 , N

χ2 =

F02 , N

1 2 π0 = C01 πkk (0) = −C02 πkk (0)

(9.158) Following Wu et al. [32], ξ = σth . In addition, I 1 , I 2 , χ 2 , and π0 may be determined to complete the characterization of the shear-enhanced volumetric strain response. Finally, we mention that the shear travel effect is determined by use of (9.130). In an effort to describe the experimental data for concrete obtained by Scavuzzo et al. [31], the endochronic equations presented for the hydrostatic, deviatoric, shear-enhanced volumetric strain, and pressure-enhanced shear strain were solved by Wu and Aboutorabi [28] in an iterative incremental fashion utilizing a computer. The increment in stress path is input into a program that computes from it an increment for the hydrostatic stress and one for the deviatoric stress. Then, accordingly, the hydrostatic and deviatoric modules are called on to ﬁnd the corresponding increment of strains and increment of intrinsic time. If any coupling strains are to be evaluated, then the increments of the intrinsic times are passed on to the shear-enhanced volumetric strain and pressure-enhanced shear strain modules to ﬁnd such strains. Any

© 2005 by Chapman & Hall/CRC Press

502

Continuum Mechanics and Plasticity 100 Principal Stress (MPa)

(a)

Theory Experiment si

4k

1

50

= 1 si 8k

=

3

2

2,3 0 0

100 Principal Stress (MPa)

(b)

2

4 6 8 10 Principal Strain (*1000)

12

Theory Experiment

50

1 4

0 –5

0 4. .5 2 .5 = 3 1 2 = 1 8 6

2,3

0 5 10 Principal Strain (*1000)

15

FIGURE 9.17 Behavior of concrete subjected to various stress paths — inserts show stress paths (From Wu, H.C. and Aboutorabi, M.R., Int. J. Plasticity, 4, 163, 1988. With permission from Elsevier).

stress path that is neither purely hydrostatic nor deviatoric is approximated by a staircase path (i.e., as a series of consecutive hydrostatic and deviatoric increments). The outputs of the theoretical computations are presented in [28]. They constitute a rather extensive study of various stress paths. It is fair to say that the model has done a good job in describing such a diverse loading program. In Figure 9.17(a) and (b), we show two cases. For each stress path the stress–strain relations in both 1- (vertical) and 2-directions are presented. The 1-direction is marked with ◦ and the 2-direction with . Since the tests are all performed in the deviatoric plane, the loadings in the 2- and 3-directions are the same and the result for the 3-direction is identical to that for the 2-direction.

9.4.3

Application to Sand

Sand is a cohesionless soil. It has mechanical properties similar to those described in the introductory paragraphs of Section 9.4. They are the hydrostatic response, the deviatoric response, the shear-enhanced volumetric response, and the hydrostatic pressure-enhanced shear response. In the

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

503

terminology of soil mechanics, the hydrostatic response is known as isotropic consolidation. The volumetric stress–strain curve bends toward the stress axis. The deviatoric behavior depends on hydrostatic stress (or the normal stress) and the deviatoric (or shear) stress–strain curve bends toward the strain axis. There is no shear strength at zero conﬁning pressure. The shear-enhanced volumetric response is also known as densiﬁcation or dilation. The ﬁrst application of the endochronic theory to the description of mechanical behavior of sand was due to Bazant and Krizek [33], using the simple endochronic theory (see Section 8.4.2). Valanis and his coworkers [34,35] have also contributed extensively to this subject. Our approach is different from aforementioned works in that we use the Gibbs formulation. The equations are similar to those presented in Section 9.4.1. Using this formulation, Wu and Wang [36] obtained theoretical results of isotropic consolidation and deviatoric response, which compare favorably with experimental results of Lade [37] for Sacramento River sand subjected to loading–unloading. In addition, the shear hysteretic loops for loose crystal silica No. 20 sand reported in [38] were theoretically investigated in [36]. We [36] also investigated densiﬁcation and the results compared favorably with those reported in [39]. The shear hysteresis of sand was further investigated by Wu and Sheu [40] using a method of integration similar to that discussed in Section 8.4.5.2, resulting in closed-form solutions. The theory predicted the test results of Silver and Seed [41] at the 1st, 2nd, 10th, and 300th cycles reasonably well. Nine cases of relative densities and vertical stresses were considered. Additional works in the endochronic modeling of sand are Wu et al. [32] considering a true triaxial test and Wu and Aboutorabi [42] considering sand behavior subjected to a circular stress path. Furthermore, the undrained response of sand was discussed in [29].

9.4.4

Application to Porous Aluminum

Recent developments in the techniques of powder metallurgy (P/M) have made it possible to solidify all kinds of metallic powders into structure components of controlled porosity. Application of endochronic theory to describe the phenomenological behavior of porous aluminum was carried out by Aboutorabi et al. [43], and Wang and Wu [44]. However, these applications were limited to isotropic consolidation and monotonic uniaxial straining, using the experimental results of Schock et al. [45] and some limited experimental data for high-purity aluminum P/M. Using specimens of high-purity aluminum P/M, Wu et al. [46] conducted a series of experiments under various cyclic straining conditions and showed that the endochronic theory presented in Section 9.4.1 can be used to describe the experimental results reasonably well. The theory of Section 9.4.1 has four elements. They are the hydrostatic response, the deviatoric response, the densiﬁcation, and the shear travel. Although densiﬁcation and shear travel are two important coupled behaviors

© 2005 by Chapman & Hall/CRC Press

504

Continuum Mechanics and Plasticity

between hydrostatic and deviatoric elements, their determination cannot be accomplished by uniaxial stress experiments and awaits further investigation by use of other specimen conﬁgurations and loading conditions. In [46], these two effects are neglected, and the efforts have been focused on the evaluation of the hydrostatic and deviatoric behaviors subjected to cyclic loading. Due to consistent results obtained even with this approximation, it may be concluded that densiﬁcation and shear travel are of secondary importance for the material tested under uniaxial stress condition. The decomposition of the axial stress–strain curve into volumetric and deviatoric stress–strain curves gives further insight into the material behavior. This is of special importance due to the signiﬁcant role played by the plastic volumetric deformation. The hydrostatic and deviatoric elements of the endochronic theory are now discussed separately and concepts of the present formulation are interpreted in terms of those of the classical plasticity. In a uniaxial strain-controlled test, the strain and stress states are ε1 0 0 σ1 0 0 [ε] = 0 ε2 0 , (9.159) [σ ] = 0 0 0 0 0 0 0 0 ε2 where 1 is in the axial direction of the cylindrical specimen. The volumetric strain is εv = ε1 + 2ε2 and the mean stress is σkk = σ1 /3. The deviatoric strain and stress are 2 0 0 3 (ε1 − ε2 ) , [e] = 0 − 13 (ε1 − ε2 ) 0 1 0 0 − 3 (ε1 − ε2 ) (9.160) 2 0 0 3 σ1 [σ ] = − 31 σ1 0 1 0 − 3 σ1 The hydrostatic response is described by (9.133) and (9.134). Several cyclic straining paths were tested. One of them is shown in Figure 9.18(a) and another in Figure 9.18(b). Both theoretical and experimental results are shown in the ﬁgures. Only one internal variable p is used for simplicity in the discus = −2σ = −2σ and e = sion of the deviatoric response. Since we have σ11 11 22 33 −2e22 = −2e33 , only the 11-components of (9.146) and (9.125) are independent equations. Combing these equations and (9.123) with kD = 1, we obtain de11 [1 ± XD ] =

dσ11 [1 ± k2 XD ] 2G0

(9.161)

where " XD =

© 2005 by Chapman & Hall/CRC Press

3 C2 (C2 σ11 − F2 p11 ) 2 f N2

(9.162)

Topics in Endochronic Plasticity

505

30

(a)

Theory Experiment

Hydrostatic Stress (MPa)

20 10 0 –10 –20 –30 –0.15

–0.05

0.05

0.15

0.25

Volumetric Strain (%) (b)

25

Theory Experiment

20 Hydrostatic Stress (MPa)

15 10 5 0 –5 –10 –15 –20 –25 0.00

0.05

0.10

0.15

0.20

0.25

Volumetric Strain (%) FIGURE 9.18 Cyclic volumetric stress–strain curve for porous aluminum: (a) test program 1, (b) test program 2 (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

The hardening function is f (zD ) = CD − (CD − 1) exp(−µzD )

(9.163)

Equations (9.161) and (9.163) are used in a numerical procedure to compute the deviatoric stress–strain curves. Figures 9.19(a) and (b) are the deviatoric counterparts of Figures 9.18(a) and (b).

© 2005 by Chapman & Hall/CRC Press

506

Continuum Mechanics and Plasticity 50

Deviatoric Stress (MPa)

(a)

Theory Experiment

25

0

–25

–50 –1 –0.8 –0.6 –0.4 –0.2 0

0.2 0.4 0.6 0.8

1

Deviatoric Strain (%) 50

Deviatoric Stress (MPa)

(b)

Theory Experiment

25

0

–25

–50 0

0.2

0.4

0.6

0.8

1

Deviatoric Strain (%)

FIGURE 9.19 Deviatoric counterparts of Figure 9.18 (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

9.5 9.5.1

An Endochronic Formulation of a Plastically Deformed Damaged Continuum Introduction

Typical work in continuum damage mechanics (CDM) often involves the damage-effect variables in the sense of Kachanov [47] and the effective stress/effective strain concepts. Consequently, damage mechanics theories are often derived from the usual constitutive theories by use of effective variables, which take into account the effects of damage, in place of

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

507

original variables. The thermodynamics framework of CDM often involves the concept of either the strain equivalence postulate [48] or the strain-energy equivalence postulate [49,50], or the hypothesis of stress working equivalence [51] along with the concepts of continuum mechanics and irreversible changes in the material internal structure. The microdefects are represented at the macroscopic level by a damage variable. A typical elastoplastic damage theory is based on the generalized damage theory initially proposed by Chaboche [52] and later by Lemaitre [53]. In [53], Lemaitre proposed that the damage energy release rate, that is, energy release by the system during the damaging process, is related to the elastic strain energy. The damage energy release rate is deﬁned by the thermodynamic force conjugate to damage evolution. This treatment amounts to an uncoupled consideration between plasticity and damage processes. These concepts of CDM have been proposed by different authors associated with different deﬁnitions and theories, and not all of them are needed in one theory. Some of the aforementioned concepts and deﬁnitions are not even compatible with each other. Following the work of Wu and Nanakorn [54], we discuss the existing concepts of CDM and propose a CDM constitutive framework using a set of concepts in a uniﬁed manner. The reproduction of [54] is with permission from Elsevier. Further constitutive modeling is required to arrive at explicit constitutive equations for CDM, which may be achieved by use of a concept such as damage potential within the proposed constitutive framework. Another approach is to formulate the constitutive equations based on an endochronic concept and still using the same constitutive framework. The endochronic formulation for CDM is discussed in this section.

9.5.2

The Anisotropic Damage Tensor

This work uses a second-order tensor as a parameter of damage. The tensor deﬁnes the loss of net area of material as in the original work of Kachanov [47]. The presentation of damage tensor Dij in this section follows previous work by Murakami and Ohno [55] and Betten [56], in which the damage tensor is constructed using area vectors related to Cauchy’s tetrahedron in a damaged state. In Murakami and Ohno’s anisotropic damage theory of creep, the second-rank symmetric damage tensor Dij is derived by representing the effects of microscopic grain-boundary cavities in terms of a dyadic product of the unit normal vector to the relevant boundary. On the other hand, in a macroscopic approach, Betten derived the damage tensor from a third-order, skew-symmetric, continuity tensor that represents the area vector. In [54], the derivation of Dij is similar to Betten’s derivation, but a second-order continuity tensor is used, which provides a simple and more meaningful physical interpretation. Consider a differential tetrahedron of an undamaged material as shown in Figure 9.20(a). Note that the ﬁgure shows a special case where xi axes coincide (j) with the principal damage axes. In general, if dSi denotes the i-component of

© 2005 by Chapman & Hall/CRC Press

508

Continuum Mechanics and Plasticity x3

(a)

(b)

x3

(4) dSi

dx3

– (4)

dSi = dSi(4)

dx3

(1)

– (1)

dSi

dSi x2

(2)

x2

– (2)

dx2

dSi

dSi

dx1

dx2 dx1

x1

(3) dSi

– (3) (3) dSi = dSi

x3

(c)

(4)

(4)

dSi = ij dSi

dx3 (1)

dSi

x2 (2) dSi

dx2 dx1

x1

– (3)

(3)

dSi = dSi

FIGURE 9.20 Deﬁnition of damage measure-load bearing area: (a) undamaged continuum, (b) actual damaged continuum, (c) ﬁctitious undamaged continuum (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

(j)

(j)

a gross area element that has the normal nk , then dSi can be characterized by (1)

= − 12 eijk dxj dxk

(2)

= − 12 eijk dxj dxk

(3)

= − 12 eijk dxj dxk

(4)

= − 12 eijk (dxj

dSi dSi dSi

(2)

(3)

(3)

(1)

(1)

(2)

(1)

dSi

(9.164) (3)

(2)

(3)

− dxj )(dxk − dxk ) (j)

where eijk is the permutation tensor and the vectors dxi do not coincide with the principal damage axes in the general case. The sum of these vectors is zero due to closure of the surface area of tetrahedron, that is (1)

dSi

© 2005 by Chapman & Hall/CRC Press

(2)

+ dSi

(3)

+ dSi

(4)

+ dSi

= 0i

(9.165)

Topics in Endochronic Plasticity

509

Consider now a tetrahedron of a material with internal damage as shown in Figure 9.20(b). The nominal dimensions of this tetrahedron are the same as those for Figure 9.20(a), but the areas are reduced by scalar factors α, β, γ , and κ from the previous tetrahedron with their corresponding normals unchanged. Then, the area vectors are (1)

= − 12 αijk dxj dxk = α dSi

(2)

= − 12 βijk dxj dxk = β dSi

(3)

= − 12 γijk dxj dxk = γ dSi

(4)

= − 12 κijk (dxj

dS¯ i dS¯ i dS¯ i dS¯ i

(2)

(3)

(1)

(3)

(1)

(2)

(1)

(2)

(3)

(1)

(3)

(9.166)

(2)

(3)

(4)

− dxj )(dxk − dxk ) = κ dSi

where αijk = αeijk , βijk = βeijk , γijk = γ eijk , and κijk = κeijk . The areas in (9.166) represent net cross-sectional areas of the element. These are the areas that are effectively resisting loads and are perpendicular to the coordinate (4) axes x1 , x2 , and x3 , respectively. Note that dS¯ i denotes the inclined side. The parameters α, β, and γ are discussed further later in this section. We (1) (4) note that the vectors dS¯ i , . . . , dS¯ i , deﬁned in (9.166), and the correspond(1) (4) ing dSi , . . . , dSi deﬁned in (9.164), differ in length, and the condition of closure cannot be satisﬁed, that is (1)

dS¯ i

(2)

+ dS¯ i

(3)

+ dS¯ i

(4)

+ dS¯ i

= 0i

(9.167)

except for the case of isotropic damage where α = β = γ = κ. Because of the existence of microcavities in the material, the load-carrying net areas of the damaged continuum, Figure 9.20(b), are reduced. It is now postulated that there exists a ﬁctitious undamaged continuum, as shown in Figure 9.20(c), which is mechanically equivalent to the damaged continuum. Thus, the damage state is represented by the ﬁctitious undamaged continuum such that (1)

= − 12 eijk dˆxj dˆxj

(2)

= − 12 eijk dˆxj dˆxj

(3)

= − 12 eijk dˆxj dˆxj

(4)

= − 12 eijk (dˆxj

dSˆ i dSˆ i dSˆ i dSˆ i

© 2005 by Chapman & Hall/CRC Press

(2)

(3)

(1) = dS¯ i

(3)

(1)

(2) = dS¯ i

(1)

(2)

= dS¯ i

(1)

(9.168)

(3)

(3)

(2)

(3)

− dˆxj )(dˆxk − dˆxk )

510

Continuum Mechanics and Plasticity (j)

where dˆxi deﬁne the ﬁctitious differential tetrahedron. Furthermore, the closure of the ﬁctitious undamaged continuum is assumed to be satisﬁed. Thus, (1)

dSˆ i

(2)

+ dSˆ i

(3)

+ dSˆ i

(4)

+ dSˆ i

= 0i

(9.169)

(j) (j) The three area vectors dSˆ i in (9.168) are identical to the vectors dS¯ i (j) in (9.166) and are related to the vectors dSi in (9.164) by scalar factors (4) (4) α, β, and γ , respectively. The fourth vectors dSˆ i and dS¯ i are different in both magnitude and direction. Since (9.168) is used in the remaining part of this chapter, the parameter κ is not important and is not discussed further. (4) (4) It is reasonable to assume that dSˆ i and dSi are related by a linear relation (4)

dSˆ i

(4)

= ψij dSj

(9.170)

(4) where ψij is a second-order tensor. In (9.170), dSˆ i represents the effective (4) load-carrying area of the damaged material and dSj is the gross area on the inclined face of the material element. Therefore, tensor ψij represents the (4) fraction of dSj that can be used to carry load, accounting for the effect of damage. Tensor ψij is known as the continuity tensor, since it describes the continuity state of the material. The continuity tensor ψij can be determined directly from (9.170). Substituting (9.164) and (9.165) into the right-hand side of (9.170), and (9.166), (9.168), and (9.169) into the left-hand side of (9.170), we obtain (2)

(3)

(3)

(1)

(1)

(2)

αijk dxj dxk + βijk dxj dxk + γijk dxj dxk (2)

(3)

(3)

(1)

(1)

(2)

= ψir erjk (dxj dxk + dxj dxk + dxj dxk )

(9.171)

(j)

If the vectors dxi are aligned with the coordinate axes xi , respectively, then (j)

dxi

= δij |ds j | (no sum on j), where |ds j | deﬁnes the magnitude of the (j)

vector dxi . Then, for i = 1, (9.171) becomes (ψ11 − α)e123 |ds2 ||ds3 | + ψ12 e231 |ds3 ||ds1 | + ψ13 e321 |ds1 ||ds2 | = 0 (9.172) (j)

Since |ds j |, the magnitudes of dxi , are independent of each other, they can be independently varied. But, due to the closure assumption, (9.172) cannot be violated. Therefore, (9.172) can be satisﬁed for all values of |ds j |, if and only if ψ11 = α,

© 2005 by Chapman & Hall/CRC Press

ψ12 = 0,

ψ13 = 0

(9.173)

Topics in Endochronic Plasticity

511

Similar discussions may be used for i = 2 and 3. Thus, the continuity tensor is found to be α 0 0 (9.174) [ψ] = 0 β 0 0 0 γ It is seen that when the xi axes are principal damage axes, the continuity tensor ψij is in a diagonal form. In the case of uniaxial tension along the x1 direction, let s be the total gross cross-sectional area and sˆ be the effective area of resistance so that sˆ < s. (4) (4) In view of (9.170), vectors dSˆ i and dSi are represented by [ˆs, 0, 0]T (4) and [s, 0, 0]T , respectively, with ni = [1, 0, 0]T . Then, by use of (9.174), (9.170) reduces to sˆ = ψs

(9.175)

where ψ = ψ11 = α. Therefore, ψ = sˆ/s represents that fraction of the crosssectional area which can be used to resist load. When ψ = 1, the material is in the virgin state without damage and sˆ is identical to s. When ψ = 0, the material can no longer resist load, since its effective area of resistance is reduced to zero. The damage tensor is deﬁned as a complementary (dual) tensor of continuity [57]. In other words, the damage tensor represents the fraction of the cross-sectional area that was reduced by microdefects. In the uniaxial loading case, the damage variable can be expressed in terms of the continuity variable ψ as D=

s − sˆ =1−ψ s

(9.176)

Thus, D = 0 corresponds to the undamaged state and D = 1 corresponds to the breaking state of the material. In the multiaxial case, a second-order damage tensor Dij is deﬁned as Dij = δij − ψij

(9.177)

Note that Dij is the damage tensor and is not to be confused with the rate of deformation tensor used in most chapters of this book. In the special case, when the xi axes are also the principal axes of damage, tensor ψij is given by (9.174), and the damage tensor is given by

D1 [D] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 D2 0

0 1−α 0= 0 0 D3

0 1−β 0

0 0 1−γ

(9.178)

512

Continuum Mechanics and Plasticity

It is seen that the principal values D1 , D2 , and D3 are related to the principal continuity variables α, β, and γ , respectively. These principal values Di can be measured on the test specimens cut along mutually perpendicular directions x1 , x2 , and x3 , respectively. Alternatively, the continuity tensor is given in terms of the principal values of the damage tensor as

α [ψ] = 0 0

0 β 0

0 1 − D1 0 = 0 γ 0

0 1 − D2 0

0 0 1 − D3

(9.179)

where α = 1 − D1 , β = 1 − D2 , and γ = 1 − D3 .

9.5.3

Gross Stress, Net Stress, and Effective Stress

In the previous section, a deﬁnition of damage is derived by introducing a ﬁctitious undamaged continuum that is mechanically equivalent to the actual damaged continuum. In this section, various deﬁnitions of stress, such as the gross stress, the net stress, and the effective stress, are discussed. The gross stress or the Cauchy stress, σij , is the stress deﬁned on the actual damaged continuum while the net stress, σˆ ij , and the effective stress, σ˜ ij , are the nonsymmetric and symmetric stress, respectively, deﬁned on the ﬁctitious undamaged continuum. By considering the actual damaged continuum and the ﬁctitious undamaged continuum under the same applied force, the corresponding stresses on the two continua are different, since the stresses are calculated over different cross-sectional areas of the continua. If the equilibrium of the actual damaged continuum is considered (Figure 9.21(a)), one can derive the relation between the stress vector ti and the stress tensor σij , that is, ti = σji nj

(9.180)

where ni is the unit normal of an area element dS. Similarly, the equilibrium of the ﬁctitious undamaged continuum, with an area element dSˆ and unit normal nˆ i (Figure 9.21(b)) yields tˆi = σˆ ji nˆ j

(9.181)

where σˆ ij is the net stress acting on the ﬁctitious undamaged continuum and tˆi is the corresponding stress vector. Since the area elements dS and dSˆ are subjected to the same force, that is, dPˆ i = dPi , we can conclude that dPi = ti dS = σji nj dS = σˆ ki nˆ k dSˆ = tˆi dSˆ = dPˆ i

© 2005 by Chapman & Hall/CRC Press

(9.182)

Topics in Endochronic Plasticity x3

(a)

513 (b)

dPi

dx3

x3

dPi = dPi

dx3

ni

21

ni

21 x2

x2

dx2

22 23

dx2

22

dx1

23

x1

(c)

x3

dx1

x1

~ dPi

dx3

~ n n i = i

21 x2 dx2

22

23

dx1

x1

FIGURE 9.21 Deﬁnitions of stress tensor and pseudo-force: (a) Cauchy stress, (b) net stress, (c) effective stress (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

where dS and dSˆ are scalar quantities and the corresponding vector expression is obtained from (9.170) as nˆ i dSˆ = ψij nj dS. Thus, (9.182) becomes (σji − σˆ ki ψkj )nj dS = 0

(9.183)

and it follows that σij = ψki σˆ kj

and

σˆ ij = ψik−1 σkj

(9.184)

By use of (9.174), the net-stress σˆ ij is found to be σ

11

α σ21 [σˆ ] = β σ31 γ

σ12 α σ22 β σ32 γ

σ13 α σ23 β σ33

(9.185)

γ

which shows that the net-stress σˆ ij is nonsymmetric, except for the case of isotropic damage. It is not convenient to use the nonsymmetric stress

© 2005 by Chapman & Hall/CRC Press

514

Continuum Mechanics and Plasticity

tensor σˆ ij together with a symmetric strain tensor and strain rate in the constitutive equations. Therefore, new symmetric stress measures, the effective stress σ˜ ij , have been deﬁned on the ﬁctitious undamaged continuum and used in the constitutive equations. Various deﬁnitions have been proposed to symmetrize σˆ ij . These deﬁnitions may be summarized based on various transformations operated on the net stress σˆ ij . They are 1. Betten [56] proposed a transformed net-stress tensor, which is an effective stress subjected to the following transformation σ˜ ij = 12 (σˆ ij ψkj−1 + ψki−1 σˆ jk )

(9.186)

Using (9.184), the expression becomes −1 σ˜ ij = 12 (ψik−1 ψij−1 + ψjk−1 ψmi )σkm = Mijkm σkm

(9.187)

where −1 Mijkm = 12 (ψik−1 ψij−1 + ψjk−1 ψmi )

(9.188)

The fourth-order transformation tensor Mijkm is referred to as the damage-effect tensor. For ψij to have the diagonalized form of (9.174), (9.187) is expressed in the matrix form as

1 α2 σ˜ 11 σ˜ 22 σ˜ 33 = σ˜ 12 σ˜ 23 σ˜ 31

0 1 β2

0

0

0

0

0

0

1 γ2

0

0

1 αβ

0

sym

1 βγ

0 0 σ11 σ22 0 σ33 σ12 0 σ23 σ31 0 1 γα

(9.189)

or σ11 α2

σ12 [σ˜ ] = αβ σ 13 αγ which is a symmetric tensor.

© 2005 by Chapman & Hall/CRC Press

σ12 αβ σ22 β2 σ23 βγ

σ13 αγ σ23 βγ σ33 γ2

(9.190)

Topics in Endochronic Plasticity

515

2. The effective stress proposed by Cordebois and Sidoroff [58], also by Chow and Wang [59], is deﬁned through its components given by σ˜ ij =

# σˆ ij σˆ ji

(no sum on i or j)

(9.191)

Since the right-hand side of (9.191) is not a tensor operation, the effective stress σ˜ ij as deﬁned by (9.191) is not a tensor. However, in the matrix form, the above deﬁnition of effective stress can also give rise to a linear relationship between σ˜ ij and σij . 3. In a study of anisotropic damage in ductile solids, Stumvoll and Swobada [60] deﬁned the effective stress as the symmetric part of the net-stress tensor, that is, −1 σ˜ ij = 12 (σ˜ ij + σ˜ ji ) = 12 (ψik−1 δjm + δik ψjm )σkm

(9.192)

where the damage-effect tensor is −1 ) Mijkm = 12 (ψik−1 δjm + δik ψjm

(9.193)

By use of (9.179), Mijkm may be written in terms of the principal damage D1 , D2 , and D3 and it can be reduced to a form used by Rabotnov [61] and later by Chow and Lu [62]. In all cases, the effective stress σ˜ ij is related to the Cauchy stress σij by the equation σ˜ ij = Mijkm σkm

(9.194)

where the exact expression for the damage-effect tensor Mijkm depends on the method used in symmetrizing σˆ ij . With respect to the principal damage coordinate system, the damage-effect tensor Mijkm is represented by a 6 × 6 diagonal matrix. In a special case, if the directions of principal stresses coincide with those of the principal damage, then these equations further reduce to σ˜ 11 0 0 M1111 σ11 σ˜ 22 = 0 M2222 0 σ22 (9.195) σ˜ 33 σ33 0 0 M3333 where M1111 , M2222 , and M3333 are functions of principal damage variables D1 , D2 , and D3 . The interpretation of the effective stress is now investigated. The net-stress tensor σˆ ij is an actual nonsymmetric stress acting on the ﬁctitious, undamaged continuum, which is subjected to the same applied force as the original, actual,

© 2005 by Chapman & Hall/CRC Press

516

Continuum Mechanics and Plasticity

damaged continuum, that is, dPˆ i = dPi . On the other hand, the effective stress tensor σ˜ ij is the ﬁctitious symmetric stress acting on the ﬁctitious undamaged continuum due to the application of the pseudo-force dP˜ i , as shown in Figure 9.21(c). To validate this statement, the Cauchy formula, relating the pseudo-force dP˜ i to the effective stress σ˜ ij is dP˜ i = σ˜ ji nˆ dSˆ

(9.196)

where nˆ i and dSˆ were previously deﬁned on the ﬁctitious undamaged element. Using (9.170) and (9.194), the above relation can be rewritten in terms of the Cauchy stress and the area element ni dS as dP˜ i = Mjikm σkm nˆ j dSˆ = Mjikm σkm ψjr nr dS

(9.197)

If Betten’s deﬁnition of the damage-effect tensor (9.188) is used, (9.197) becomes dP˜ i = ψij−1 dPj

(9.198)

This equation establishes that the pseudo-force dP˜ i is related to the original applied force dPi by the inverse-transpose of the continuity tensor ψij . If, on the other hand, the damage-effect tensor is deﬁned by (9.193), then the pseudo-force on the ﬁctitious undamaged element is ˆ = 1 (dPi + ψ −1 σjk nˆ j dS) ˆ dP˜ i = 12 (dPi + σˆ ij nˆ j dS) 2 ik

(9.199)

ˆ due to the nonsymmetric property We note that dPi = σˆ ji nˆ j dSˆ = σˆ ij nˆ j dS, of σˆ ij . The last term of (9.199) can be viewed as an additional abstract-force due to the actual stress σij acting over the area of the ﬁctitious undamaged ˆ Therefore, the pseudo-force corresponding to this continuum, that is, nˆ j dS. deﬁnition of effective stress has no simple physical interpretation. 9.5.4

An Internal State Variables Theory

Based upon concepts of continuum mechanics and irreversible thermodynamics with internal variables, the Clausius–Duhem inequality (with thermal gradient) with respect to the actual, damaged continuum is given by (see [63]) ˙ ij , qrij , Dij , γijs , θ) − ηθ˙ − σij ε˙ ij − (ε

1 hj θ,j ≥ 0 θ

(9.200)

In (9.200), the Helmholtz free energy is a function of total (elastoplastic) strain εij , damage measure Dij , temperature θ, and two sets of internal

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

517

state variables qrij and γijs . There are n number of internal variables qrij (r = 1, 2, . . . , n), which describe the state of plastic deformation, and m number of internal variables γijs (s = 1, 2, . . . , m), which specify the state of damage in the continuum. hi is heat ﬂux vector and η is entropy density. In a typical damage mechanics model, the damage tensor Dij is treated as an internal state variable (it is macroscopically not measurable by deﬁnition) that describes the irreversible process of internal structure due to microdefects. However, in the present work, the damage tensor Dij is not an internal state variable and it represents a measurable quantity, that is, the fraction of reduction in load-resisting area. It is a measurable quantity in the description of damage, even though it may be difﬁcult to measure. The role played by Dij in the description of damage is similar to the role played by strain, which is also measurable, in the description of plastic deformation. In [54], a set of internal state variables γijs has been introduced to describe the state of internal damage as a result of growth and/or nucleation of microcracks and/or microvoids. The set of m internal variables γijs , which evolves with loading histories, is introduced to distinguish one internal state of damage from the others, similar to the set of internal variables qrij which describes the state of plastic deformation that cannot be uniquely described by the plastic strain alone. The damage variable Dij describes the current fraction of area reduction but not the state of damage. To elaborate, two continua of the same initial damaged state, when undergoing different loading histories, may end up having the same load-resisting area momentarily, hence the same value of Dij , but having two different states of damage. The concept of using both damage tensor Dij and damage internal state variables γijs in [54] is similar but not equal to the concept of Krajcinovic [64] proposed for the brittle CDM model. In Krajcinovic’s model, the microcracks vector ﬁelds ω(i) , treated as internal variables, are used to describe the state of damage, and a scalar damage measure D is used to describe the overall damage of the material. However, D is the macroscopic counterpart of the microscopic ω(i) (they are related by an integral) and D is, therefore, not measurable. In the present work, Dij is deﬁned by a deﬁnition not directly related to γijs and it is inﬂuenced by the current loading condition. Thus, at the same state of damage, a different incremental loading state will give rise to a different increment of Dij . Hence, dDij is different when the material element is subjected to incremental tension, compression, or shear. As an illustration, consider uniaxial tension of a cylinder. The majority of the microcracks will develop in the plane perpendicular to the maximum tensile strain. If the specimen is then unloaded and subsequently subjected to a small compressive stress along its axial direction, the specimen will behave as though it were undamaged up to a certain compressive stress threshold, since all of the microcracks will be passive (crack closure). Consequently, the initial increment of Dij depends on whether the stress increment is tensile or compressive, even though the state of damage is the same at that moment. Furthermore, with the second-order tensor representations of Dij and γijs , the theory [54] is capable of describing both spherical (e.g., void volume fraction) and

© 2005 by Chapman & Hall/CRC Press

518

Continuum Mechanics and Plasticity

planar (e.g., a system of planar microcracks) effects of microcracks, and their interactions. In the ﬁctitious undamaged conﬁguration, the volume and surface area of the continuum are reduced by excluding the volume and area of the continuum that were previously occupied by microdefects. These are denoted by ˆ and S, ˆ respectively. Consequently, the ﬁctitious undamaged matrix material V becomes homogeneous and isotropic. For a given force ﬁeld Pˆ i = Pi , the ﬁrst law of thermodynamics written for this ﬁctitious undamaged continuum is 1 d ˆ ˆ ˆ ˆ ˆ ˆ ρˆ bi vˆ i dV + (σˆ ji vˆ i − hj )nˆ j dS + rˆ dV vˆ i vˆ i + εˆ ρˆ dV = dt Vˆ 2 ˆ ˆ V Sˆ V (9.201) where ( ∧ ) is used to indicate that the quantity is associated with the ﬁctitious undamaged continuum. In (9.201), vˆ i is the velocity; εˆ is the internal energy density; ρˆ is the mass density; bˆ i is the body force; and rˆ is the heat source term. The ﬁrst term in the surface integral represents the rate of work done by surface traction and is expressed in terms of the nonsymmetric netstress tensor σˆ ij . When the pseudo-force ﬁeld P˜ i is introduced to the ﬁctitious continuum so that the corresponding effective stress σ˜ ij is symmetric, (9.201) is written as d 1 ˆ ˆ ˆ ˆ = ˆ ˆ ˜ ˜ ˜vi v˜ i + εˆ ρˆ dV ˆ rˆ dV ρˆ bi vi dV + (σ˜ ji vi − hj )nj dS + dt Vˆ 2 ˆ ˆ V Sˆ V (9.202) Due to the use of pseudo-force ﬁeld P˜ i , the velocity vector in this conﬁguration is v˜ i instead of vˆ i , as indicated in (9.202). Consequently, the deformation of the ﬁctitious undamaged continuum subjected to pseudo-force ﬁeld P˜ i is different from that subjected to force ﬁeld Pi . The rate of deformation for the ﬁctitious undamaged conﬁguration is then deﬁned by ∂ v˜ ˙ε˜ ij = 1 ∂ v˜ i + j (9.203) 2 ∂xj ∂xi where ε˜ ij deﬁnes the deformation of the ﬁctitious undamaged continuum (with pseudo-force ﬁeld P˜ i ) and is referred to as the effective strain. According to (9.203), the relationship between the effective strain ε˜ ij and the actual strain εij depends on transformations between velocity vectors from vi to vˆ i and from vˆ i to v˜ i . In general, the explicit forms of these transformations are difﬁcult to deﬁne due to the complexity of the geometry and mathematics involved. In this work, the effective strain ε˜ ij is expressed in terms of damage tensor Dij and actual strain εij , and this relationship is discussed later in this section. The postulate of free energy equivalence is applied in the subsequent discussion. According to this postulate, which was initially proposed

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

519

by Cordebois and Sidoroff [58] in the form of strain-energy equivalence, the free energy for an actual, damaged material has the same form as that for a ﬁctitious, undamaged material, but the variables are replaced by the effective quantities. Thus, ˜ ε˜ ij , q˜ rij , γijs , θ ≡ εij , qrij , Dij , γijs , θ (9.204) where the q˜ rij ’s are the effective qrij ’s. Note that Dij does not explicitly appear as one of the state variables on the left-hand side of (9.204). In view of (9.204), the free energy available to do mechanical work and stored in the ﬁctitious continuum is the same as that stored in the actual continuum, resulting in an equivalent mechanical behavior. The second law of thermodynamics and the equation of motion at the ﬁctitious conﬁguration subjected to the pseudo-force ﬁeld P˜ i become d dt

ˆ V

ˆ ≥ ρη ˆ dV

ˆ V

rˆ ˆ dV − θ

ˆ hi nˆ j dSˆ Sˆ θ

∂ σ˜ ji + ρˆ bˆ i = ρˆ f˜i ∂xi

(9.205) (9.206)

where fˆi = d˜vi /dt. Using (9.202) to (9.206), the Clausius–Duhem inequality for the ﬁctitious undamaged continuum in the isothermal condition is given by ˙˜ ε˜ , q˜ r , γ s ≥ 0 σ˜ ij ε˙˜ ij − (9.207) ij ij ij so that

˜ ∂ σ˜ ij − ∂ ε˜ ij

˜ ˜ s ∂ ∂ ε˙˜ ij − r q˙˜ rij − γ˙ ≥ 0 ∂ q˜ ij ∂γijs ij

(9.208)

In the ﬁctitious continuum, ε˜ ij , q˜ rij , and γijs are the state variables so that they can be independently varied. Although, q˜ rij may vary when ε˜ ij changes, their relation is not one-to-one. Different ε˜ ij histories may lead to the same q˜ rij , and a material with different q˜ rij may correspond to the same ε˜ ij momentarily. Thus, it is possible to vary ε˜ ij so that q˜ rij is left unchanged. Therefore, inequality (9.208) is always satisﬁed, if σ˜ ij =

˜ ∂ ∂ ε˜ ij

and

−

˜ r ˜ s ∂ ∂ γ˙ ≥ 0 q˙˜ ij − r ∂ q˜ ij ∂γijs ij

(9.209)

According to the ﬁrst equation of (9.209), the effective stress σ˜ ij is derivable ˜ The inequality (9.209) gives the from the ﬁctitious undamaged free-energy . thermodynamic constraints on the laws governing the evolution of the two sets of internal variables, q˜ rij and γijs .

© 2005 by Chapman & Hall/CRC Press

520

Continuum Mechanics and Plasticity

It is now possible to derive the explicit relationship for effective strain ε˜ ij . A relation similar to the ﬁrst equation of (9.209) exists for the actual damaged continuum. When the postulate of free energy equivalence is assumed, this relation is σij =

˜ ˜ ∂ ε˜ mn ˜ ∂ q˜ rmn ∂ ∂ ∂ ∂ = = + r ∂εij ∂εij ∂ ε˜ mn ∂εij ∂ q˜ mn ∂εij

(9.210)

where the effective internal variable q˜ rij is assumed to be a function of the actual internal variable qrij and damage tensor Dij . Note that, for the actual damaged continuum s independent variables are εij , qrij , and Dij , so that the second term on the right-hand side of (9.210) drops out and the equation reduces to σij =

˜ ∂ ε˜ mn ∂ ε˜ mn ∂ = σ˜ mn ∂ ε˜ mn ∂εij ∂εij

(9.211)

Using (9.194), (9.211) further reduces to ∂ ε˜ mn = Nijmn ∂εij

(9.212)

where Nijmn is the inverse of Mijmn and is a function of Dij only, or Mijmn Nrsij = Imnrs

(9.213)

In (9.213), the fourth-order identity tensor is Iijkm = δik δjm and δij is Kronecker’s delta. Thus, it follows from (9.212) that the effective strain ε˜ ij is linearly related to εij by ε˜ ij = Nkmij εkm

or

εij = Mkmij ε˜ km

(9.214)

Then, it is assumed that the following relations are valid for the internal variable qrij q˜ rij = Nkmij qrkm

or

qrij = Mkmij q˜ rkm

(9.215)

Constitutive equations at the ﬁctitious undamaged conﬁguration must satisfy the inequality given by (9.207). By use of (9.214) this inequality can be written as ˙˜ ε , q˜ r , γ s ) + σ˜ ∂ ε˜ km D ˙ ij ≥ 0 σij ε˙ ij − (˜ ij ij ij km ∂Dij

(9.216)

∂ ε˜ ij ∂Nrsij = εrs ∂Dmn ∂Dmn

(9.217)

where

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

521

By observing (9.204), the ﬁrst two terms of (9.216) are the same as the lefthand side of (9.200) in the isothermal case. During an incremental loading, the ﬁctitious undamaged continuum undergoes a deformation in the matrix as well as an increase in damage. The ﬁrst two terms of (9.216) are energy dissipated associated with this process. However, by deﬁnition, the state of the ﬁctitious material remains undamaged at the end of each loading increment. The amount of energy dissipated in order to restore the ﬁctitious continuum to the undamaged state is represented by the last term of inequality (9.216). For convenience, inequality (9.216) can be rewritten as ˙˜ ε˜ , q˜ r , γ s − G D ˙ σij ε˙ ij − ij ij ij ij ij ≥ 0

(9.218)

where Gij = −σ˜ km

∂ ε˜ km ∂Dij

(9.219)

Tensor Gij is the thermodynamic force associated with unit damage growth ˙ ij , and, in this work, it is referred to as the “damage force” for simplicity. This D quantity may also be considered as the energy release rate per unit damage advance. Physically, the negative of the damage force, −Gij , can be interpreted as the “restoring force” that restores the ﬁctitious continuum to its undamaged ˙ ij . It is seen from (9.219) that state after experiencing a unit damage growth D Gij can be expressed in terms of σ˜ ij , ε˜ ij , and Dij . A further discussion of the damage force can be found in the appendix of [54].

9.5.5

Plasticity and Damage

We now characterize the plastic deformation process, the damage process, and the coupling between the two processes. Starting with the actual damaged conﬁguration, where the state variables are εij , Dij , qrij , and γijs , the Clausius– Duhem inequality (9.200) can be rewritten for isothermal process as σij ε˙ ij −

∂ ∂ ∂ ˙ ∂ s Dij − ε˙ ij − r q˙ rij − γ˙ ≥ 0 ∂εij ∂qij ∂Dij ∂γijs ij

(9.220)

˜ and noting that Dij and γ s are independent variables, (9.220) Replacing by ij becomes ˜ ∂ ε˜ ij ˜ ∂ q˜ rij r ˜ ∂ ε˜ ij ˜ ∂ q˜ rij ∂ ∂ ∂ ∂ ˙ km σij ε˙ ij − D ε˙ km − r r q˙ km − + r ∂ ε˜ ij ∂εkm ∂ q˜ ij ∂qkm ∂ ε˜ ij ∂Dkm ∂ q˜ ij ∂Dkm −

˜ s ∂ γ˙ ≥ 0 ∂γijs ij

© 2005 by Chapman & Hall/CRC Press

(9.221)

522

Continuum Mechanics and Plasticity

or, after regrouping of terms, it may be shown that ˙˜ ε˜ , q˜ r , γ s ≥ 0 σij ε˙ ij − ij ij ij

(9.222)

Constraint (9.222) represents the Clausius–Duhem inequality of the actual damaged conﬁguration. However, unlike (9.200), inequality (9.222) involves ˜ εij , q˜ r , γ s ), which is deﬁned in the ﬁctithe ﬁctitious free energy (˜ ij ij tious undamaged conﬁguration, where the ﬁctitious material is isotropic. ˜ εij , q˜ r , γ s ) involves only material constants that are isotropic Therefore, (˜ ij ij tensors. In an attempt to characterize the plastic deformation and the damage process, one recognizes that the damage process does not directly inﬂuence the mechanisms of plastic deformation; that is, there is no direct coupling between damage and plastic deformation. In general, plasticity is directly related to slips for metals and to other mechanisms for other materials. In all cases, damage inﬂuences plastic strains only because the net area of resistance decreases as the damage proceeds. In the present work, damage does not directly inﬂuence plastic deformation of the ﬁctitious undamaged continuum, but it does inﬂuence the plastic deformation of the actual continuum. Based on this ˜ εij , q˜ r , γ s ) is assumed to consist of observation, the ﬁctitious free energy (˜ ij ij ˜ 1 (˜εij , q˜ r ) and the damage potential two parts, the ﬁctitious plastic potential ij ˜ 2 (Dij , γ s ), that is, ij

˜ ε˜ ij , q˜ rij , γijs = ˜ 1 ε˜ ij , q˜ rij + ˜ 2 Dij , γijs

(9.223)

˜ 1 (˜εij , q˜ r ) characterizes the plastic process of the ﬁctitious where potential ij ˜ 2 (Dij , γ s ) describes the damage undamaged continuum while potential ij process. During deformation, the microcracks and microvoids will extend, grow, and nucleate, resulting in progressive material deterioration. This damage deterioration is not arbitrary and it must obey thermodynamic ˜ 2 (Dij , γ s ) is used to constraints to be established. The damage potential ij provide the equation of damage evolution and its necessary constraints. The state of microdefects is represented by the set of internal variables γijs . The change in microdefects together with the loading condition bring about a decrease in load-resisting area, which is represented at the macroscopic level by damage tensor Dij . The effect is carried over to the deformation process, elastic or plastic, through the effective variables, σ˜ ij , ε˜ ij , and q˜ rij . Hence, an indirect coupling occurs between the plasticity and damage in the actual damaged continuum. Using (9.223), inequality (9.222) is written as ˙˜ D , γ s ≥ 0 ˙˜ ε˜ , q˜ r − σij ε˙ ij − ij ij 1 ij ij 2

© 2005 by Chapman & Hall/CRC Press

(9.224)

Topics in Endochronic Plasticity 9.5.6

523

The Constitutive Equations and Constraints

Within an inﬁnitesimal strain theory, the stress rate is usually represented by the material rate. In CDM, it is important, however, to consider the rotation of the principal directions of damage during the deformation process. The principal directions of damage do not generally coincide with the principal stress, when nonproportional loading takes place or when the material has suffered a prior damage. To satisfy the requirements of reference frame indifference, the rate of change of damage measure Dij and the internal variables γijs are expressed by the corotational derivatives ˙ D∇ ij = Dij − ωik Dkj + Dik ωkj ,

γijs∇ = γ˙ijs − ωik γkjs + γiks ωkj

(9.225)

where ωij represents the spin of the principal damage coordinate frame with respect to the ﬁxed reference coordinate frame. Thus, it follows from (9.224) that ˜ 1 ∂ ε˜ km ˜ 1 ∂ q˜ rkm r ∂ ∂ σij − ε˙ ij − r q˙ ∂ ε˜ km ∂εij ∂ q˜ km ∂qrij ij ˜ 1 ∂ q˜ rkm ˜2 ˜ s∇ ˜ 1 ∂ ε˜ km ∂ ∂ ∂ ∂ D∇ + r + γ ≥0 (9.226) − ij − ∂ ε˜ km ∂Dij ∂ q˜ km ∂Dij ∂Dij ∂γijs ij Since εij , Dij , qrij , and γijs are independent state variables, ﬁxing these values ˜ 1 , and ˜ 2 because they are state functions. For also ﬁx the values of σij , inequality (9.226) not to be violated for any arbitrary choice of ε˙ ij while keeping Dij , qrij , and γijs unchanged, the following conditions must hold σij =

˜ 1 ∂ ε˜ km ∂ , ∂ ε˜ km ∂εij ˜ 1 ∂ q˜ rkm r ∂ − r q˙ − ∂ q˜ km ∂qrij ij

(9.227a)

˜ 1 ∂ ε˜ km ˜ 1 ∂ q˜ rkm ˜2 ∂ ∂ ∂ + r + ∂ ε˜ km ∂Dij ∂ q˜ km ∂Dij ∂Dij

D∇ ij −

˜ s∇ ∂ γ ≥0 ∂γijs ij (9.227b)

Using (9.212) and noting that Nijkm is the inverse of Mijkm , (9.227a) reduces to σ˜ ij =

˜1 ∂ ∂ ε˜ ij

(9.228)

˜ 1 (˜εij , q˜ r ). Also, (9.227b) Thus, the effective stress is derivable from potential ij can be rearranged to yield ˜ 1 r∇ ˜2 ˜ 2 s∇ ∂ ∂ ∂ − r q˜ km + Gij − D∇ γ ≥0 ij − ∂ q˜ km ∂Dij ∂γijs ij

© 2005 by Chapman & Hall/CRC Press

(9.229)

524

Continuum Mechanics and Plasticity

where Gij =

˜ 1 ∂ ε˜ km ∂ ε˜ km ∂ = −σ˜ km ∂ ε˜ km ∂Dij ∂Dij

(9.230)

In the derivation, (9.228) and (9.219) were used. Note that the ﬁrst term of (9.227b) and the second term in the bracket of the same inequality are combined to form the ﬁrst term of (9.229). From the assumption that damage does not directly inﬂuence the state of ﬁctitious plasticity, that is, damage affects the deformation only through Dij , the constraint (9.229) can be replaced by the following stronger conditions ˜1 ∂ − r q˜ r∇ ≥0 ∂ q˜ ij ij

˜2 ∂ Gij − ∂Dij

and

D∇ ij −

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.231)

The conditions apply, respectively, to the ﬁctitious plastic deformation process and the damage process. Furthermore, if the values of εij , Dij , qrij , and γijs ˜ 2 are also ﬁxed, since Gij is a function of are ﬁxed, then the values of Gij and ˜ 2 is a state function. For inequalstate variables as deﬁned by (9.230), and ity (9.231b) not to be violated for an arbitrary choice of D∇ ij , the following conditions must hold Gij =

˜2 ∂ ∂Dij

and

−

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.232)

For a more detailed investigation of a CDM model, the damage tensor Dij can be divided into two parts, that is, Dij = Drij + Dnij

(9.233)

The recoverable part Drij is due to area reduction associated with the growth of microdefects that can be recovered during unloading. The nonrecoverable part Dnij involves the reduction of area due to the extension of existing microcracks and/or the nucleation of microdefects. In summary, the constitutive equations for an isothermal damaged continuum are given by the following sets of equations and constraints σ˜ ij =

˜1 ∂ ∂ ε˜ ij

with −

˜ 1 r∇ ∂ q˜ ≥ 0 ∂ q˜ rij ij

(9.234)

Gij =

˜2 ∂ ∂Dij

with −

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.235)

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

525

and Gij = −

˜ 1 ∂ ε˜ km ∂ ∂ ε˜ km ∂Dij

(9.236)

Equation (9.234) characterizes the deformation of the ﬁctitious undamaged continuum, and the inequality of (9.234) constrains the evolution of plastic internal variables. The set of equation and constraint (9.235) provides a relationship between the damage force Gij and the damage measure Dij . It also provides a constraint on the evolution of damage internal variables. Finally, the coupling between the deformation process and damage process is provided by (9.236). This is further explained in the subsequent paragraph. Consider a ﬁctitious, undamaged, element subjected to loading increment ˜ dPi . During loading, there are various forms of dissipation of energy associated with plasticity and damage processes. In particular, the rate of energy dissipation (caused by the damage force) due to a unit damage growth D∇ ij ∇ ˜ with respect to the ﬁctitious element is (∂ 2 /∂Dij )D . At the end of the loadij

ing period, it is required that the ﬁctitious element returns to its undamaged state before the next loading can be applied. The restoring energy associated with this transformation is given by −Gij D∇ ij , where −Gij is the restoring force. Because the damage needed to be restored at the end of a loading period is equal to the negative of the damage growth during loading, the force associated with the two processes must be equal in magnitude. Therefore, (9.236) can be viewed as a constraint that must be satisﬁed for the ﬁctitious deformation and damage process to occur simultaneously within the same continuum. In fact, this is a required constraint that arrives naturally from thermodynamic consideration. Equations and constraints in (9.234) to (9.236) provide a framework for theories of CDM. Explicit constitutive equations may be obtained if functions ˜ 1 and ˜ 2 are speciﬁed. Explicit evolution equations, which satisfy the for inequalities of (9.234) and (9.235), for internal variables qrij , and γijs should also be given. Different theories may be proposed based on this constitutive framework. One such theory has been formulated by Wu and Nanakorn [65] by use of the concept of endochronic plasticity. In that paper, the model has been applied to a one-dimensional case that describes uniaxial monotonic compression and tension of a concrete specimen. It successfully describes the strain-softening behavior after the peak load. In addition, the model has been applied to the description of deformation behavior for cyclically loaded concrete and mortar specimens. Satisfactory results have been obtained. It is remarked that the internal variables are not observable. Using the evolution equations for these variables, these variables do not necessarily appear in the ﬁnal form of the constitutive equations. Depending on the functional ˜ 1 and ˜ 2 and the explicit forms for the evolution equations for qr , forms for ij and γijs , a set of macroscopic parameters may be used for the model. These parameters may then be determined from experiments.

© 2005 by Chapman & Hall/CRC Press

526

Continuum Mechanics and Plasticity

9.5.7

A Brief Summary of Wu and Nanakorn’s Endochronic CDM

Several CDM models based on endochronic theory of plasticity have been proposed. The model of Valanis [66] is for brittle materials, while the models of Niu [67] and Chow and Chen [68] are for ductile materials. The model of Niu [67] is limited to isotropic damage due to the scalar representation of damage; the model of Chow and Chen [68] is an anisotropic damage model. Wu and Nanakorn’s model [65] is applicable to ductile materials with anisotropic damage. The equations of the Wu–Nanakorn model are summarized in this section for later references with permission from ASCE. This model is different from that of Chow and Chen [68], which uses neither the damage internal variables γijs nor the concept of damage restoring force Gij . Instead, Chow and Chen [68] uses Dij as an internal variable and express the damage evolution equations in terms of the potential of damage dissipation and elastic strain energy release rate Yij . In the Wu–Nanakorn model, the governing equations and constraints are given by (9.234) to (9.236). In this section, explicit forms of equations ˜ 1 (˜εij , q˜ r ) and are derived by assuming the following quadratic forms for ij ˜ 2 (Dij , γ s ): ij

1 ˜ 1 ε˜ ij , q˜ rij = Aijkm ε˜ ij − q˜ rij ε˜ km − q˜ rkm 2 r

1 s ˜ 2 Dij , γijs = Hijkm Dij − γijs Dkm − γkm 2 r

(9.237) (9.238)

where Aijkm and Hijkm are positive semi-deﬁnite fourth-rank isotropic tensors. The free energies in (9.237) and (9.238) are deﬁned on the ﬁctitious undamaged material, which is isotropic. Represent now any fourth-order isotropic tensor Wijkm by W2 Wijkm = W1 δij δkm + W2 δik δjm , with W0 = 3 W1 + (9.239) 3 where W1 and W2 are constants, and symmetry of Wijkm with respect to k and m is assumed. Also, the variables may be decomposed into the deviatoric and hydrostatic parts as σ˜ ij = σ˜ ij + 13 δij σ˜ kk ,

ε˜ ij = e˜ij + 13 δij ε˜ kk ,

q˜ rij = p˜ ijr + 13 δij q˜ rkk

(9.240)

and Gij = gij + 13 δij Gkk ,

Dij = dij + 13 δij Dkk ,

s γijs = rijs + 13 δij γkk

(9.241)

Using these notations, the explicit form of constitutive equations for damaged materials may be derived and are presented in the remaining part of this section.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

527

9.5.7.1 Equations of plastic deformation The deformation behavior is characterized by the effective stress-effective strain relationship given in (9.234). Using (9.237), this equation reduces to the following two equations by separating hydrostatic and deviatoric components: σ˜ kk =

Ar0 (˜εkk − q˜ rkk )

(9.242)

Ar2 (˜eij − p˜ ijr )

(9.243)

r

σ˜ ij =

r

where Ar0 and Ar2 are deﬁned by (9.239) with W replaced by A. Within a linear assumption, the evolution equations for the hydrostatic and deviatoric parts of q˜ rij are given in the following form Lr0

d˜qrkk d˜zH

∇ − σ˜ kk = 0

and

Lr2

d˜pijr d˜zD

∇ − σ˜ ij = 0

(9.244)

where ( )∇ indicates that the differentiation operator in bracket is corotational; Lr0 and Lr2 are constants; and d˜z deﬁnes the intrinsic time with respect to the ﬁctitious deformation. The intrinsic time is divided into the hydrostatic and deviatoric parts. An hydrostatic intrinsic time measure ζH is deﬁned to register the hydrostatic deformation. It is scaled by the intrinsic time scale zH so that it can properly describe strain hardening. They are related by $ $ $ dσ˜ kk $$ $ dζH = $d˜εkk − k1 3K $

with

0

dζH = h (ζH ) > 0 dzH

(9.245)

where 0 ≤ k1 ≤ 1 and K0 is the Bulk Modulus. The deviatoric intrinsic time ˜ ij which is given by ζD is deﬁned based on an effective strain-like tensor Q ˜ ij =∇ d˜eij − k2 dQ

∇

∇dσ ˜ ij

2µ0

(9.246)

where 0 ≤ k2 ≤ 1 and µ0 is the shear modulus. The operator ∇d denotes the corotational increment and is deﬁned on a second-order tensor aij with respect to the intrinsic time z as ∇

daij = t daij − Wik akj dz + aik Wkj dz

(9.247)

where t d denotes the increment based on material rate and Wij is the spin tensor. The deviatoric intrinsic time is deﬁned and scaled as follows: ˜ ij ∇ dQ ˜ ij dζD2 = ∇dQ

© 2005 by Chapman & Hall/CRC Press

with

dζD = f (ζD ) > 0 dzD

(9.248)

528

Continuum Mechanics and Plasticity

In (9.245) and (9.248), h(ζH ) and f (ζD ) are the strain-hardening functions corresponding to the hydrostatic and deviatoric deformation, respectively. 9.5.7.2 Equations of damage Equations (9.235) and (9.238) lead to the following relations for the hydrostatic and deviatoric parts of damage force Gij , respectively, Gkk =

s H0s Dkk − γkk ,

gij =

s

H2s dij − rijs

(9.249)

s

where H0s and H2s are constants. In the hydrostatic damage, microdefects expand and contract such that the overall symmetric properties of the material, that is, all planes of symmetry, are retained. In the deviatoric damage, the orientation of microcracks and microvoids changes, resulting in changes of overall symmetry properties and inducing the anisotropic behavior of the material. Using the inequality of (9.235), the linear evolution equations of γijs can be further separated into hydrostatic and deviatoric parts as J0s

s dγkk d dzH

∇

− Gkk = 0

and

J2s

drijs d dzD

∇ − gij = 0

(9.250)

d and dzd are the damage intrinsic time where J0s and J2s are constants; dzH D increment corresponding to the hydrostatic and deviatoric damage, respectively. The hydrostatic damage intrinsic time and its timescale are deﬁned, respectively, by

$ $ $ dGkk $$ d = $$dDkk − k3 dζH 3B $ 0

with

d dζH d dzH

d = hd ζH >0

(9.251)

where 0 ≤ k3 ≤ 1 and B0 is a material constant. Similarly, the deviatoric damage intrinsic time and its timescale are deﬁned by d 2 dζD = ∇dRij ∇dRij

with

= f d ζDd > 0

dζDd d dzD

(9.252)

where the damage-like tensor ∇dRij is deﬁned by ∇

dRij = ∇ddij − k4

∇dg

ij

2M0

(9.253)

with 0 ≤ k4 ≤ 1 and M0 is a material constant. The role played by material constants B0 and M0 in the Gij versus Dij relationship is similar to that played

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

529

by the bulk modulus K0 and shear modulus µ0 in the stress–strain relationd ) and f d (ζ d ) describe the material damage resisting ship. The functions hd (ζH D (hardening) behavior, which increases the damage threshold. These functions are similar to the hardening functions h(ζH ) and f (ζD ) of plastic deformation, but with a different physical meaning. The role played by (9.251) and (9.252) in damage is analogous to that played by (9.245) and (9.248) in the stress–strain space for the limit case of ki → 1 (i = 1, 2, 3, 4). The relations (9.251a) and (9.253) can be interpreted as the nonrecoverable hydrostatic and deviatoric parts of the damage tensor increment dDij , respectively. Note that ζ d is deﬁned in terms of the nonrecoverable damp age Dnij rather than the effective plastic strain ε˜ ij , as in the theories of Niu [67] and Chow and Chen [68]. This new damage intrinsic time enables the present theory to describe the behavior of damage in brittle materials, where damage occurs within the elastic range, as well as in ductile materials. 9.5.7.3

Coupling between deformation and damage

The coupling between deformation and damage processes is achieved through the damage force Gij given by (9.236). Using the quadratic form of ˜ 1 (˜εij , q˜ r ) given in (9.237), (9.236) reduces to ij

∂ ε˜ uv ∇ ) ∂Dij r dNpquv ∇ =− Aruvmn ε˜ mn − q˜ rmn εpq dDij r

Gij = −

Aruvmn (˜εmn − q˜ rmn )(

(9.254)

This equation relates the damage force Gij to the effective strain ε˜ ij and effective internal variables q˜ rij , both of which are responsible for the deformation process of the ﬁctitious continuum. On the other hand, the damage force is ˜ 2 (Dij , γ s ) by (9.235), which, by use of (9.238), related to the damage potential ij reduces to Gij =

˜2 ∂ s s Dkm − γkm = Hijkm ∂Dij s

(9.255)

This equation relates damage force Gij to the damage tensor Dij and internal variables γijs . The interpretations of (9.254) and (9.255) are as follows: consider a ﬁctitious, undamaged, material element subjected to a loading increment. During loading, different forms of energy associated with plasticity and damage process are dissipated. In particular, the rate of energy dissipation ∇ due to damage growth D∇ ij in the ﬁctitious element is (∂2 /∂Dij )Dij . At the end of the loading period, it is required that the ﬁctitious element returns to its undamaged state before the next loading can be applied. The restoring energy

© 2005 by Chapman & Hall/CRC Press

530

Continuum Mechanics and Plasticity

associated with this process is −Gij D∇ ij , where −Gij is the restoring force and the negative of the restoring force, Gij , is given by (9.254). Because the damage to be restored at the end of the loading period is equal to the negative of the damage growth during loading, the force associated with the two processes must be equal in magnitude. Therefore, (9.255) with Gij deﬁned by (9.254), can be viewed as a constraint that must be satisﬁed for the deformation and damage processes to occur simultaneously within the ﬁctitious continuum. In fact, this is a required constraint which arises naturally from the thermodynamic consideration. 9.5.8

Application

In this section, the model of the previous section is applied to investigate the problem of a cylindrical concrete specimen subjected to uniaxial compression in the x3 -direction. For such a problem, the state of stress and strain is given by 0 0 0 0 ε11 0 [σ ] = 0 0 0 [ε] = 0 ε22 0 (9.256) 0 0 σ33 0 0 ε33 where ε33 is prescribed for a strain control test. These are the principal stress and strain components and the directions of principal damage coincide with those of the principal stress and strain, if the specimen is initially isotropic and is subjected to proportional loading. In this case, the corotational rate reduces to the material rate. The increments of effective stress and effective strain are 0 0 0 0 0 d˜ε11 0 d˜ε22 0 [dσ˜ ] = 0 0 [d˜ε ] = 0 (9.257) 0 0 dσ˜ 33 0 0 d˜ε33 Their deviatoric parts are 0 0 −dσ˜ 33 1 −dσ˜ 33 0 [dσ˜ ] = 0 3 0 0 2 dσ˜ 33 0 (2 d˜ε11 − d˜ε22 −d˜ε33 ) 1 0 (−d˜ε11 + 2 d˜ε22 [d˜e] = −d˜ε33 ) 3 0 0

0

0 (−d˜ε11 − d˜ε22 +2 d˜ε33 )

(9.258)

The damage-effect tensor Mijkm is selected according to Betten’s deﬁnition of effective stress. Using (9.179) and (9.188), this tensor and its inverse are

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

531

expressed in the matrix form as

1 (1 − D1 )2 0 [M] = 0 [N] =

(1 − D1 )2

0

0

1 (1 − D2 )2

0

0

1 (1 − D3 )2

(9.259)

(1 − D2 )2

(1 − D3 )2

where D1 , D2 , and D3 are the principal damage in the x1 , x2 , and x3 directions, respectively. In this example, for the sake of simplicity, only one internal variable each for q˜ ij and γij is used. The use of only one internal variable was shown in previous applications of endochronic plasticity to be capable of capturing the main features of stress–strain responses in a plastically deformed continuum. The hydrostatic behavior of the ﬁctitious deformation is now considered. Combining (9.242), (9.244a) and (9.245a), the following equation is obtained dσ˜ kk dσ˜ kk ± k1 X = (1 ± X)d˜εkk A0 3K0

with X =

σ˜ kk L0 h(ζH )

(9.260)

where A0 and L0 are constants. The minus (−) and plus (+) signs, in (9.260), correspond to tension and compression, respectively. The material constant A0 may be identiﬁed with the bulk modulus 3K0 by considering the ﬁctitious undamaged material at its initial loading state, where σ˜ kk = q˜ kk = 0. Using the effective stress and effective strain of (9.257), (9.260) becomes dσ˜ 33 = 3K0 F(k1 , X)(d˜ε11 + d˜ε22 + d˜ε33 )

(9.261)

σ˜ 33 L0 h(ζH )

(9.262)

where F(k1 , X) =

1±X 1 ± k1 X

and

X=

The deviatoric response of the ﬁctitious undamaged material, from (9.243), (9.244b), and (9.258), is described by A2 σ˜ 33 dzD L2 A2 σ˜ 33 − dσ˜ 33 = A2 (−d˜ε11 + 2 d˜ε22 − d˜ε33 ) + dzD L2 A2 σ˜ 33 2 dσ˜ 33 = A2 (−d˜ε11 − d˜ε22 + 2 d˜ε33 ) − dzD L2 − dσ˜ 33 = A2 (2 d˜ε11 − d˜ε22 − d˜ε33 ) +

© 2005 by Chapman & Hall/CRC Press

(9.263a) (9.263b) (9.263c)

532

Continuum Mechanics and Plasticity

Equation (9.261) and the two independent equations of (9.263) can be put in the matrix form as 1 −3K0 F(k1 , X) −3K0 F(k1 , X) dσ˜ 33 0 1 d˜ε11 + 1 A2 σ˜ 33 dzD 2A2 −A2 L2 1 1 −A2 2A2 d˜ε22 3K0 F(k1 , X) d˜ε33 A2 = (9.264) A2 where dzD is related to the deviatoric components of the incremental effective strain d˜εij and its relationship is now discussed. The following expression may be found from (9.246) ˜ ij = ϕij + ψij dzD dQ

(9.265)

where ϕij = (1 − k2 )d˜eij

and

ψij =

k2 σ˜ ij

(9.266)

L2

By use of (9.248) and (9.265), the relation for dzD is obtained as 2 ϕij ϕij + 2ϕij ψij dzD + [ψij ψij − f (ζD )2 ]dzD =0

(9.267)

The equation of hydrostatic damage is found from (9.249a), (9.250a), and (9.251a) as dGkk dGkk ± k3 Y = (1 ± Y) dDkk H0 3B0

with Y =

Gkk d) J0 hd (ζH

(9.268)

where H0 , B0 , and J0 are material constants. Considering the initial loading state, where Gkk = γkk = 0, it may be shown that H0 is the initial slope of the Gkk versus Dkk curve and that H0 = 3B0 . The minus (−) and plus (+) signs, in (9.268), correspond to tension and compression, respectively. Equation (9.268a) further reduces to dGkk = H0 F(k3 , Y) dDkk

with F(k3 , Y) =

1±Y 1 ± k3 Y

(9.269)

The equation for deviatoric damage response may be obtained from (9.249b) and (9.250b) as gij d dgij = H2 ddij + dzD J2

© 2005 by Chapman & Hall/CRC Press

(9.270)

Topics in Endochronic Plasticity

533

where H2 and J2 are constants and H2 may be identiﬁed with the initial slope of the deviatoric Gij versus Dij curve. Furthermore, H2 = 2M0 . The damd is related to the deviatoric components of age intrinsic time increment dzD the damage force increment dgij and its relationship is now discussed. The following expression may be found from (9.253) and (9.270) d dRij = ϕijd + ψijd dzD

(9.271)

where ϕijd = (1 − k4 )

dgij H2

and

ψijd =

gij J2

(9.272)

d is obtained as By use of (9.252a) and (9.271), the relation for dzD

d 2 d + ψijd ψijd − f d (ζDd )2 (dzD ) =0 ϕijd ϕijd + 2ϕijd ψijd dzD

(9.273)

Using (9.236) and (9.257), the damage force Gij reduces to Gij = −σ˜ km

∂ ε˜ km ∂ ε˜ 33 = −σ˜ 33 ∂Dij ∂Dij

(9.274)

Since ε˜ 33 = (1 − D3 )2 ε33 , ε˜ 33 does not depend on D1 and D2 . Consequently, the only nonzero component of tensor Gij is G33 =

2σ˜ 33 ε˜ 33 1 − D3

(9.275)

and its increment is found to be dG33 =

2σ˜ 33 2˜ε33 2σ˜ 33 ε˜ 33 d˜ε33 + dσ˜ 33 + dD3 1 − D3 1 − D3 (1 − D3 )2

(9.276)

Thus, the deviatoric part of the increment of the damage force is

−dG33 1 [dgij ] = 0 3 0

0 −dG33 0

0 0 2dG33

(9.277)

Furthermore, 0 0 2 dD1 − dD2 − dD3 1 0 0 −dD1 + 2 dD2 − dD3 [ddij ] = 3 0 0 −dD1 − dD2 + 2 dD3 (9.278)

© 2005 by Chapman & Hall/CRC Press

534

Continuum Mechanics and Plasticity

Equations (9.277) and (9.278) are substituted into (105) and the two independent equations of (9.269) to obtain the following matrix equation for the damage process:

H0 F(k3 , Y) H0 F(k3 , Y) H0 F(k3 , Y) dD1 2H2 −H2 −H2 dD2 −H2 2H2 −H2 dD3 1 0 H2 G33 d = −1 dG33 − 1 dzD J2 −1 1

(9.279)

The equations derived in this section are now applied to the problem of uniaxial compression of cylindrical concrete specimen (fc = 73.8 MPa and E=27.6 GPa). To determine the material parameters for the model, the analytical stress–strain curves obtained by Fonseka and Krajcinovic [69] is used. In this case, the directions of the principal damage coincide with those of the principal stress. The procedure of calculation is now described. An increment d˜ε33 is ﬁrst speciﬁed. An initial value for dzD is assumed and (9.264) solved for dσ˜ 33 , d˜ε11 , and d˜ε22 . These values are then used in (9.267) to solve for dzD . An iteration procedure is applied to determine dG33 . (9.273) d . Thus, dD , dD , and dD are found is subsequently used to determine dzD 1 2 3 from (9.279). An iteration procedure is also applied on dD3 to determine its value, which corresponds to the speciﬁed d˜ε33 . Knowing d˜ε33 and dD3 , dε33 can be calculated from the incremental form of ε33 =

ε˜ 33 (1 − D3 )2

(9.280)

This procedure continues for another speciﬁed d˜ε33 . Using a trial-and-error (curve-ﬁtting) procedure, the following material parameters for the deformation equations have been determined: Poisson’s ratio = 0.2, effective hydrostatic yield stress L0 = 4.55 MPa, effective deviatoric yield stress L2 = 18.61 MPa, strain-hardening parameters µH = µd = 0, and k1 = k2 = 0.95. The material parameters for the damage equations have been found to be: hydrostatic damage modulus H0 = 0.78 MPa, deviatoric damage modulus H2 = 1.91 MPa, hydrostatic damage threshold J0 = 0.61 MPa, deviatoric damage threshold J2 = 1.93 MPa, damage resisting (hardening) parameters µdH = µdD = 0, and k3 = k4 = 0.95. The computed stress–strain curves are plotted in Figure 9.22. There are two curves in this ﬁgure. One curve is for the axial strain and the other for the lateral strain. The volumetric strain versus compressive stress is plotted in Figure 9.23. The curve shows a change of sign of the volumetric strain as the axial strain increases. The volumetric strain is initially negative and it changes to positive when the axial strain becomes large in magnitude. This phenomenon is typical in concrete and rocks, and it is due to the increase

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

535 Compressive stress (MPa)

60 40 Endochronic 20 Fonseka and Krajcinovic (1981) Strain (%) –0.2

–0.4

0.2

Axial Strain

Lateral Strain

FIGURE 9.22 Stress versus axial and lateral strains in uniaxial compression of concrete (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

Compressive Stress (MPa) Endochronic Fonseka and Krajcinovic (1981)

60 40 20

–0.1

–0.05

0.05

0.1

Volumetric Strain (%) FIGURE 9.23 Stress versus volumetric strain in uniaxial compression of concrete (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

in the lateral-to-axial strain ratio (−ε11 /ε33 ) as the axial strain increases. It is seen in Figure 9.24 that this ratio changes from 0.2 to approximately 0.6 as the axial compressive strain increases from 0 to 0.005. The results of this model presented in Figure 9.22 and Figure 9.23 show good agreement with the computed value obtained by Fonseka and Krajcinovic [69].

9.5.9

Concluding Remarks

The concepts of CDM have been discussed and a constitutive framework of CDM has been developed based on the internal variables approach. The framework involves transforming the actual damaged continuum into an equivalent ﬁctitious undamaged continuum. The effects of damage are

© 2005 by Chapman & Hall/CRC Press

Continuum Mechanics and Plasticity

The –11/33 Ratio

536

0.5 0.4 0.3 0.2 0.1

0.2

0.3

0.4

0.5

Axial strain 33 (%) FIGURE 9.24 Lateral to axial strain ratio versus axial compressive strain (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

accounted for by replacing the actual stress σij (gross stress) on the damaged continuum with the symmetric effective stress σ˜ ij . Adistinction has been made between the state of damage and the damage measure Dij and the concept of “damage force” has been introduced. Within the proposed constitutive framework, the endochronic concept has been used to derive explicit constitutive equations. Two intrinsic times are used in the formulation. The ﬁrst intrinsic time ζ is used to describe the plastic deformation history of the ﬁctitious undamaged continuum and the second intrinsic time ζ d is used to depict the damage history. The model is applicable to both brittle and ductile materials with damage. The following conclusions may be drawn from this study: 1. The damage tensor Dij may be deﬁned based on a second-order continuity tensor ψij . 2. The damage-effect tensor Mijkm deﬁned by Betten [58] gives rise to an effective stress that has a simple physical interpretation, while other deﬁnitions of Mijkm do not have the same signiﬁcance. 3. The transformation equation for effective strain, (9.214), may be derived based on the free energy equivalence postulate. 4. In addition to damage tensor Dij , which is a measurable quantity, a set of damage internal variables γijs , which are not measurable, is used in the formulation. 5. The constitutive equations for an isothermal damaged continuum include two sets of equations and constraints. The ﬁrst set characterizes the deformation of the ﬁctitious undamaged continuum and constrains the evolution of plastic internal variables qrij . The second set provides a relationship between the damage force Gij and the damage measure Dij . It also provides a constraint on the evolution of damage internal variables γijs . In addition, (9.236) must be used to complete the constitutive equations. This equation is a constraint that

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

537

must be satisﬁed for the ﬁctitious deformation and damage process to occur simultaneously within the same continuum. 6. The theory does not use the concepts of yield surface or damage surface as its prime requisite although both surfaces may be deﬁned when necessary by setting all ki = 1. Therefore, the constitutive equations of this theory are continuous without discontinuities, which is advantageous in the numerical calculation. 7. The proposed model has been shown to describe the threedimensional state of deformation of a cylindrical concrete specimen subjected to uniaxial compression. The focal point of the work of Wu and Nanakorn [54] is to formulate a constitutive framework that is self-consistent. Some well-known concepts have been discussed and it has been pointed out that some concepts are not compatible with others. Only concepts that are compatible to each other are used in the derivation. New concept such as the distinction between the state of damage and damage measure and the concept to restore the ﬁctitious continuum to its undamaged state after each step of deformation and damage have been introduced. Finally, we mention that we use the corotational rate to account for rotation of principal damage directions during deformation.

References 1. Wu, H.C. and Yeh, W.C., Some considerations in the endochronic description of anisotropic hardening, Acta Mech., 69, 59, 1987. 2. Ohashi, Y., Tokuda, M., Mitake, T., Kurita, Y., and Suzuki, T., Stress–strain relation of integral type for deformation of brass along strain trajectories consisting of three normal straight branches, Arch. Mech., 32, 125, 1980. 3. Ohashi, Y., Tokuda, M., Suzuki, T., and Kurita, Y., Stress–strain relation of brass for the plastic deformation along bi-linear strain trajectories with various corner angles, Bull. Japan. Soc. Mech. Eng., 24, 1909, 1981. 4. Wu, H.C., Hong, H.K., and Lu, J.K., An endochronic theory accounted for deformation induced anisotropy, Int. J. Plasticity, 11, 145, 1995. 5. Wu, H.C., Lu, J.K., and Pan, W.F., Endochronic equations for ﬁnite plastic deformation and application to metal tube under torsion, Int. J. Solids Struct., 32, 1079, 1995. 6. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Struct., 8, 463, 1972. 7. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 8. Wu, H.C. and Lu, J.K., Further development and application of an endochronic theory accounted for deformation induced anisotropy, Acta Mech., 109, 11, 1995.

© 2005 by Chapman & Hall/CRC Press

538

Continuum Mechanics and Plasticity

9. Wu, H.C. and Hong, H.K., Endochronic description of plastic anisotropy in sheet metal, Int. J. Solids Struct., 36, 2735, 1999. 10. Hill, R., A theory of yielding and plastic ﬂow of anisotropic materials, Proc. Roy. Soc., London, A, 193, 281, 1948. 11. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 12. Valanis, K.C., Proper tensorial formulation of the internal variable theory, The endochronic time spectrum, Arch. Mech., 29, 173, 1977. 13. Valanis, K.C., Back stress and Jaumann rates in ﬁnite plasticity, Int. J. Plasticity, 6, 353, 1990. 14. Dafalias, Y.F., Plastic spin: necessity or redundancy?, Int. J. Plasticity, 14, 909, 1998. 15. Im, S. and Atluri, S.N., A study of two ﬁnite strain plasticity models: an internal time theory using Mandel’s director concept, and a general isotropic/kinematic-hardening theory, Int. J. Plasticity, 3, 163, 1987. 16. Goddard, J.D. and Miller, C., An inverse for the Jaumann derivative and some applications to the rheology of viscoelastic ﬂuids, Rheol. Acta, 5, 177, 1966. 17. Dafalias, Y.F., Corotational integral in constitutive formulations, J. Eng. Mech., 113, 1967, 1987. 18. Swift, H.W., Length change in metal under torsional overstrain, Engineering, 163, 253, 1947. 19. Hart, E.W. and Chang, Y.W., Material rotation effects in tension–torsion test: experimental result, in Plasticity Today, Sawczuck, A. and Bianchi, G.E., Eds., Elsevier Appl. Sci., U.K., 1985, 235. 20. White, C.S., Bronkhorst, C.A., and Anand, L., An improved isotropickinematic hardening model for moderate deformation metal plasticity, Mech. Mater., 10, 127, 1990. 21. Wu, H.C. and Xu, Z.Y., An extensometer investigation of the axial effect during torsion. Proc. Int. Conf. on Constitutive Laws for Eng. Material, Fan, J. and Murakami, S., Eds., Chongqing, China, 1989, 232. 22. Bailey, J.A., Haas, S.L., and Nawab, K.C., Anisotropy in Plastic Torsion, J. Basic Eng., 94, 231, 1972. 23. Wu, H.C., Xu, Z., and Wang, P.T., Torsion test of aluminum in the large strain range, Int. J. Plasticity, 13, 873, 1998. 24. Canova, G.R., Kocks, U.F., and Jonas, J.J., Theory of torsion texture development, Acta Metall., 32, 211, 1984. 25. Taylor, G.I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc., A, 230, 323, 1932. 26. Lowe, T.C. and Lipkin, J., Analysis of axial deformation response during reverse shear, Sand90-8417, Sandia National Lab., 1990. 27. Qian, Z. and Wu, H.C., A 2-D texture study based on a double-slip model of polycrystal plasticity with analysis of thin-walled tube under torsion, Int. J. Solids Struct., 33, 4167, 1996. 28. Wu, H.C. and Aboutorabi, M.R., Endochronic modeling of coupled volumetric–deviatoric behavior of porous and granular materials, Int. J. Plasticity, 4, 163, 1988. 29. Wu, H.C., An endochronic theory for porous and granular materials, in Modern Approaches to Plasticity, Kolymbas, D., Ed., Elsevier, Amsterdam, 1993, 347.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

539

30. Johnson, J.N. and Green, S.J., Mechanical response of porous media subject to static load, in Effects of Voids on Material Deformation, Cowin, S.C. and Carroll, M.M., Eds., AMD-16, ASME, New York, 1976, 93. 31. Scavuzzo, R., Stankowski, T., Gerstle, K.H., and Ko, H.Y., Stress–strain curves for concrete under multiaxial load histories, Report, Department of Civil, Environmental and Architectural Engineering, University of Colorado, Boulder, CO, 1983. 32. Wu, H.C., Wang, Z.K., and Aboutorabi, M.R., Endochronic modeling of sand in true triaxial test, J. Eng. Mech., ASCE, 111, 1257, 1985. 33. Bazant, Z.P. and Krizek, R.J., Endochronic constitutive law for liquefaction of sand, J. Eng. Mech. Div., ASCE, 102, 225, 1976. 34. Valanis, K.C. and Read, H.E., A new endochronic plasticity model for soils, in Soil Mechanics-Transient and Cyclic Loads, Pande, G.N. and Zienkiewicz, O.C., Eds., John Wiley, New York, 1982. 35. Valanis, K.C. and Peters, J.F., Conﬁgurational plasticity in granular media, in Modern Approaches to Plasticity, Kolymbas, D., Ed., Elsevier, Amsterdam, 1993, 1. 36. Wu, H.C., Wang, T.P., Endochronic description of sand response to static loading, J. Eng. Mech., ASCE, 109, 970, 1983. 37. Lade, P.V., Elasto-plastic stress–strain theory for cohesiveless soil with curved yield surfaces, Int. J. Solids Struct., 13, 1019, 1977. 38. Cuellar, V., Bazant, Z.P., Krizek, R.J., and Silver, M.L., Densiﬁcation and hysteresis of sand under cyclic shear, J. Geotechn. Eng. Division, ASCE, 103, 399, 1977. 39. Lee, K.L. and Seed, H.B., Drained strength characteristics of sands, J. Soil Mech. Found. Div., ASCE, 93, 117, 1967. 40. Wu, H.C. and Sheu, J.C., Endochronic modeling for shear hysteresis of sand, J. Geotechn. Eng., ASCE, 109, 1539, 1983. 41. Silver, M.L. and Seed, H.B., Deformation characteristic of sand under cyclic loading, J. Soil Mech. Found. Div., ASCE, 97, 1081, 1971. 42. Wu, H.C. and Aboutorabi, M.R., Endochronic model of sand with circular stress path, J. Geotechn. Eng., ASCE, 114, 93, 1988. 43. Aboutorabi, M.R., Wu, H.C., Wang, T.P., and Gao, Q.Y., Stress–strain behavior of porous aluminum, in Proc. 2nd International Conf. on Constitutive Laws for Engineering Materials: Theory and Application, Desai, C.S., Krempl, E., Kiousis, P.D., and Kundu, T., Eds., Elsevier, New York, 1987, 477. 44. Wang, P.T. and Wu, H.C., An endochronic model for compaction of porous metals, Prog. Powder Metall., 41, 161, 1986. 45. Schock, R.N., Abey, A.E., and Duba A., Quasi-static deformation of porous beryllium and aluminum, J. Appl. Phys., 47, 53, 1976. 46. Wu, H.C., Wang, P.T., Pan, W.F., and Xu, Z.Y., Cyclic stress–strain response of porous aluminum, Int. J. Plasticity, 6, 207, 1990. 47. Kachanov, L.M., On the time to failure during creep, Izv. AN. SSSR., OTN.337,1958. 48. Lemaitre, J. and Chaboche, J.L., Aspects phénoménologique ge la rupture par endommagement, J. Méc. Appl., 2, 167, 1978. 49. Sidoroff, F., Description of anisotropic damage application to elasticity, in Physical Non-Linearities in Structure Analysis-IUTAM, Hult, J. and Lemaitre, J., Eds., Springer-Verlag, New York, 1981, 237.

© 2005 by Chapman & Hall/CRC Press

540

Continuum Mechanics and Plasticity

50. Lemaitre, J. and Chaboche, J.L., Mécanique des Matériaux Solides, Paris: Dunod; English Edition, Cambridge University Press, 1985. 51. Chow, C.L. and Lu, T.J., A comparative study of continuum damage models for crack propagation under gross yielding, Int. J. Fract., 53, 43, 1992. 52. Chaboche, J.L., Sur l’utilisation des variables d’état interne pour la description du comportement viscoplastique et de la rupture par endommagement, Symposium Franco-Polonais de Rhéologie et Mécanique, Cracovie, 1977. 53. Lemaitre, J., A continuum damage mechanics model for ductile fracture, J. Eng. Mater. Technol., 107, 83, 1985. 54. Wu, H.C. and Nanakorn, C.K., A constitutive framework of plastically deformed damaged continuum and a formulation using the endochronic concept, Int. J. Solids Struct., 36, 5057, 1999. 55. Murakami, S. and Ohno, N., A continuum theory of creep and creep damage, in Creep Structures, Ponter A.R.S. and Hayhust, D.R., Eds., Springer, Berlin, 1981, 922. 56. Betten, J., Damage tensors in continuum mechanics, J. Mecanique theorique et appliqué, 2 , 13, 1983. 57. Rabotnov, Y.N., Creep Problems in Structural Members, North-Holland Series in Applied Math. and Mech., Vol. 7, Chap. 6, North-Holland, Amsterdam,1969. 58. Cordebois, J.P. and Sidoroff, F., Damage induced elastic anisotropy, Comportement mecanique des solides anisotropes, EUROMECH, 115, Proc. Coll., Int. du C.N.R.S., Boehler J.P. Ed., Villard-de-Lens, France, 1979, 761. 59. Chow, C.L. and Wang, J., An anisotropic theory of elasticity for continuum damage mechanics. Int. J. Fract., 33, 3, 1987. 60. Stumvoll, M. and Swobada, G., Deformation behavior of ductile solids containing anisotropic damage, J. Eng. Mech., 119, 1331, 1993. 61. Rabotnov, Y.N., Creep rupture, in Proceedings, Applied Mechanics Conference, Hetenyi, M. and Vincenti, H., Eds., Standford University, 1968, 342. 62. Chow, C.L. and Lu, T.J., On evolution laws of anisotropic damage, Eng. Fract. Mech., 34, 679, 1989. 63. Valanis, K.C., Irreversible Thermodynamics of Continuous Media, Springer-Verlag, Udine, 1971. 64. Krajcinovic, D., Continuous damage mechanics revisited: basic concepts and deﬁnition, ASME, J. Appl. Mech., 52, 829, 1985. 65. Wu, H.C. and Nanakorn, C.K., An endochronic theory of continuum damage mechanics, ASCE, J. Eng. Mech., 124, 200, 1998. 66. Valanis, K.C., A theory of damage in brittle materials, Eng. Fract. Mech., 36, 403, 1990. 67. Niu, X., Endochronic plastic constitutive equations coupled with isotropic damage and damage evolution models, Eur. J. Mech., A/Solids, 8, 293, 1989. 68. Chow, C.L. and Chen, X.F., An anisotropic model of damage mechanics based on endochronic theory of plasticity, Int. J. Fract., 55, 115, 1992. 69. Fonseka, G.U. and Krajcinovic, D., The continuous damage theory of brittle materials, part 2: uniaxial and plane response modes. J. Appl. Mech., 48, 816, 1981.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

541

Problems (1) Start from (9.10) and derive (9.11). (2) Derive (9.13). (3) Show that if the intrinsic time is deﬁned by dζ 2 = dεp · K · dεp + tr(L · dεp ) dζ , then the corresponding yield function is (σ − α) · K · (σ − α) + σy f (z)tr[L · (σ − α)] = (σy f (z))2 .

(4) In (9.37), the evolution equations of internal variables qrx and qry are dqrx + Pr qrx + U r qry = Pr εx + U r εy dz dqry + Qr qry + V r qrx = Qr εy + V r εx dz where Pr , Qr , U r , and V r are not functions of qrx and qry . These two equations are coupled in qrx and qry . Decouple the equations. (5) Derive (9.45). (6) For the PG materials discussed in Section 9.4.1, derive the governing equations given by (9.127) to (9.130). (7) In the application to porous aluminum discussed in Section 9.4.4, derive (9.161) and (9.162) for the deviatoric stress–strain behavior.

© 2005 by Chapman & Hall/CRC Press

10 Anisotropic Plasticity for Sheet Metals

10.1

Introduction

Sheet metal is a special product form of a material that is produced by the rolling process. The process of rolling is illustrated by considering a strip of metal passing between a pair of rolls with their axes parallel to each other. The sheet metal enters the rolls, and the marginal speed of the rolls on the entry side is higher than the entry speed of the sheet. The friction forces created between the rolls and the metal strip tend to pull the strip into the gap between the rolls, where plastic deformation takes place. On exiting the rolls, the friction forces change direction and the sheet acquires a reduced thickness, while the speed of the sheet is greater than the speed of the rolls. The thickness of a metal sheet can be reduced further by additional rolling, generating various degrees of anisotropy. The anisotropy in the sheet metal is two-fold: the anisotropy in the yield stress and the anisotropy in the plastic ﬂow. The anisotropy is usually speciﬁed with respect to the rolling direction (RD) of the sheet (Figure 10.1); TD denotes the transverse direction and ND, the normal direction, which is not shown in the ﬁgure. Tension specimens cut at various angles θ measured counterclockwise from the rolling direction can exhibit different yield stresses and different characteristics of plastic deformation. Generally, both the yield stress and the plastic deformation are functions of the orientation angle θ . However, it is possible that a material does not show noticeable anisotropy in the yield stress but shows signiﬁcant anisotropy in the plastic deformation. The anisotropy of plastic ﬂow is usually measured by the plastic strain-ratio R, which is deﬁned by many recent researchers as p

R= p

dεw p

dεt

(10.1) p

where dεw is the plastic strain increment in the width direction, and dεt that in the thickness direction of a tension specimen. The value of R can vary from one sheet material to the other. It can be greater than one or less than one, and R = 1 implies material isotropy. The R-ratio is an important parameter 543

© 2005 by Chapman & Hall/CRC Press

544

Continuum Mechanics and Plasticity TD

RD

FIGURE 10.1 Tension specimen cut at angle θ .

of a sheet material. A large R means a small change in the thickness during longitudinal tension, while a small R corresponds to a large change in the thickness during longitudinal stretching. Therefore, a small R would lead to easy thinning and early failure of the sheet. This deﬁnition of R-ratio is not universal, however. Recent researchers prefer the deﬁnition of (10.1) because of its apparent tie to the ﬂow rule of plasticity. On the other hand, the ASTM Standards [1] deﬁne the R-ratio as R=

εw εt

where εw = ln

wf w0

and

εt = ln

tf t0

(10.2)

The subscripts ( )0 and ( )f denote the initial and ﬁnal lengths, respectively; w stands for width and t, the thickness. Thus, the R-ratio is the ratio between the true width strain and the true thickness strain. Due to the thinness of sheets, the thickness strain is difﬁcult to measure accurately. A practical method is to measure the longitudinal and width strains and make the assumption of volume constancy. Therefore, (10.2) reduces to R=

ln(w0 /wf ) ln(lf wf /l0 w0 )

(10.3)

where l is the longitudinal measurement. Many researchers believe that the R-ratio does not vary appreciably with strain and make the assumption of constancy in their theoretical analyses. Detailed information concerning the strain level at which the measurements of R were taken is generally not reported in the literature. Some measurements were taken after the specimens had undergone large deformation. Some were taken midway between the ﬁrst occurrence of nonuniform strain and the ﬁnal fracture. Tracking of the R-ratio during experiments has indicated, however, that the R-ratio may vary greatly with the increasing plastic strain [2]. Mellor [2] and Lin and Ding [3] noted further that, due to the inaccuracy of the experimental data, the R-ratio could not be assessed closer to the initial yield region of the material. The variation of R-ratio with increasing plastic strain is discussed later in this chapter.

© 2005 by Chapman & Hall/CRC Press

Anisotropic Plasticity for Sheet Metals

10.2

545

Standard Tests for Sheet Metal

10.2.1

The Uniaxial Tension Test

Tensile specimens are cut at predetermined angles θ (usually every 15◦ ) to the rolling direction. Uniaxial tension tests are conducted on these specimens and yield stress σθ determined as a function of θ. The stress state is given by σx = σθ cos2 θ ,

σy = σθ sin2 θ,

and σxy = σθ sin θ cos θ

(10.4)

After the test, strains in both the axial and width directions of the specimens are measured, and the thickness strain determined by the assumption of volume constancy.

10.2.2

Equibiaxial Tension Test

This experiment is performed to determine the equibiaxial yield stress σB . It can be accomplished by a self-designed loading frame attached to a universal test machine or a servo-hydraulic test system. When the sheet is thin and the static loading is of concern, the experiment could also be carried out by use of a self-designed dead-weight loading system. For a more versatile testing, two servo-controlled actuators may be placed 90◦ from each other to form the loading system.

10.2.3

Hydraulic Bulge Test

This test could also be used to determine the equibiaxial yield stress σB . In the bulge test, a thin disc of sheet metal is clamped around its periphery and then subjected to an increasing ﬂuid pressure applied to one side. The region in the vicinity of the dome becomes nearly spherical in shape as the sheet bulges. The tensile stresses in the plane of the sheet are the same by symmetry. An advantage of the bulge test is that it can be carried out to strains far greater than the instability strain in tension and is not complicated by friction as is the compression test. However, the test results are not direct. A boundary value problem has to be solved in which a constitutive equation is needed.

10.2.4

Through-Thickness Compression Test

Cylindrical specimens are prepared from discs of the sheet material glued together with an epoxy adhesive. The specimens were tested in compression using Teﬂon sheet and graphite grease for lubrication between the spec

© 2005 by Chapman & Hall/CRC Press

CRC S ERIES: M ODERN M ECHANICS

AND

M ATHEMATICS

Series Editors: David Gao and Ray W. Ogden

PUBLISH E D TITLE S

BEYOND PERTURBATION: INTRODUCTION

TO THE

HOMOTOPY ANALYSIS METHOD

by Shijun Liao

MECHANICS OF ELASTIC COMPOSITES by Nicolaie Dan Cristescu, Eduard-Marius Craciun, and Eugen Soós

CONTINUUM MECHANICS

AND PLASTICITY

by Han-Chin Wu

FO RTH CO MIN G TITLE S

HYBRID INCOMPATIBLE FINITE ELEMENT METHODS by Theodore H.H. Pian, Chang-Chun Wu

MICROSTRUCTURAL RANDOMNESS by Martin Ostroja Starzewski

© 2005 by Chapman & Hall/CRC Press

IN

MECHANICS

OF

MATERIALS

Continuum Mechanics and Plasticity

Han-Chin Wu

CHAPMAN & HALL/CRC A CRC Press Company Boca Raton London New York Washington, D.C.

© 2005 by Chapman & Hall/CRC Press

Library of Congress Cataloging-in-Publication Data Wu, Han-Chin. Continuum mechanics and plasticity / Han-Chin Wu. p. cm. — (Modern mechanics and mathematics series ; no. 3) Includes index. ISBN 1-58488-363-4 (alk. paper) 1. Continuum mechanics. 2. Plasticity. I. Title. II. CRC series—modern mechanics and mathematics ; 3. QA808.2.W8 2004 531—dc22

2004055118

This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. A wide variety of references are listed. Reasonable efforts have been made to publish reliable data and information, but the author and the publisher cannot assume responsibility for the validity of all materials or for the consequences of their use. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming, and recording, or by any information storage or retrieval system, without prior permission in writing from the publisher. The consent of CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from CRC Press for such copying. Direct all inquiries to CRC Press, 2000 N.W. Corporate Blvd., Boca Raton, Florida 33431. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe.

Visit the CRC Press Web site at www.crcpress.com © 2005 by Chapman & Hall/CRC Press No claim to original U.S. Government works International Standard Book Number 1-58488-363-4 Library of Congress Card Number 2004055118 Printed in the United States of America 1 2 3 4 5 6 7 8 9 0 Printed on acid-free paper

© 2005 by Chapman & Hall/CRC Press

Contents

Preface

xiii

Author

xvii

Part I

Fundamentals of Continuum Mechanics

1

Cartesian Tensors 1.1 Introduction 1.1.1 Notations 1.1.2 Cartesian Coordinate System 1.1.3 Special Tensors 1.2 Vectors 1.2.1 Base Vectors and Components 1.2.2 Vector Addition and Multiplication 1.2.3 The e–δ Identity 1.3 The Transformation of Axes 1.4 The Dyadic Product (The Tensor Product) 1.5 Cartesian Tensors 1.5.1 General Properties 1.5.2 Multiplication of Tensors 1.5.3 The Component Form and Matrices 1.5.4 Quotient Law 1.6 Rotation of a Tensor 1.6.1 Orthogonal Tensor 1.6.2 Component Form of Rotation of a Tensor 1.6.3 Some Remarks 1.7 The Isotropic Tensors 1.8 Vector and Tensor Calculus 1.8.1 Tensor Field 1.8.2 Gradient, Divergence, Curl 1.8.3 The Theorem of Gauss References Problems

3 3 3 4 4 5 5 5 6 8 12 13 13 16 18 19 20 20 22 23 28 34 34 34 37 40 41

2

Stress 2.1 Introduction 2.2 Forces

45 45 45 v

© 2005 by Chapman & Hall/CRC Press

vi

Contents 2.3 2.4 2.5 2.6 2.7 2.8 2.9

Stress Vector The Stress Tensor Equations of Equilibrium Symmetry of the Stress Tensor Principal Stresses Properties of Eigenvalues and Eigenvectors Normal and Shear Components 2.9.1 Directions Along which Normal Components of σij Are Maximized or Minimized 2.9.2 The Maximum Shear Stress 2.10 Mean and Deviatoric Stresses 2.11 Octahedral Shearing Stress 2.12 The Stress Invariants 2.13 Spectral Decomposition of a Symmetric Tensor of Rank Two 2.14 Powers of a Tensor 2.15 Cayley–Hamilton Theorem References Problems

3

Motion and Deformation 3.1 Introduction 3.2 Material and Spatial Descriptions 3.2.1 Material Description 3.2.2 Spatial Description 3.3 Description of Deformation 3.4 Deformation of a Neighborhood 3.4.1 Homogeneous Deformations 3.4.2 Nonhomogeneous Deformations 3.5 The Deformation Gradient 3.5.1 The Polar Decomposition Theorem 3.5.2 Polar Decompositions of the Deformation Gradient 3.6 The Right Cauchy–Green Deformation Tensor 3.6.1 The Physical Meaning 3.6.2 Transformation Properties of CRS 3.6.3 Eigenvalues and Eigenvectors of CRS 3.6.4 Principal Invariants of CRS 3.7 Deformation of Volume and Area of a Material Element 3.8 The Left Cauchy–Green Deformation Tensor 3.9 The Lagrangian and Eulerian Strain Tensors 3.9.1 Deﬁnitions 3.9.2 Geometric Interpretation of the Strain Components 3.9.3 The Volumetric Strain 3.10 Other Strain Measures 3.11 Material Rate of Change 3.11.1 Material Description of the Material Derivative 3.11.2 Spatial Description of the Material Derivative

© 2005 by Chapman & Hall/CRC Press

46 47 50 52 53 55 59 60 60 64 65 66 69 71 72 73 74 79 79 80 80 81 83 83 85 86 88 88 90 98 98 101 103 104 105 108 108 108 112 115 118 119 119 120

Contents

4

3.12 Dual Vectors and Dual Tensors 3.13 Velocity of a Particle Relative to a Neighboring Particle 3.14 Physical Signiﬁcance of the Rate of Deformation Tensor 3.15 Physical Signiﬁcance of the Spin Tensor 3.16 Expressions for D and W in Terms of F 3.17 Material Derivative of Strain Measures 3.18 Material Derivative of Area and Volume Elements References Problems

122 124 125 128 129 131 132 133 134

Conservation Laws and Constitutive Equation 4.1 Introduction 4.2 Bulk Material Rate of Change 4.3 Conservation Laws 4.3.1 The Conservation of Mass 4.3.2 The Conservation of Momentum 4.3.3 The Conservation of Energy 4.4 The Constitutive Laws in the Material Description 4.4.1 The Conservation of Mass 4.4.2 The Conservation of Momentum 4.4.3 The Conservation of Energy 4.5 Objective Tensors 4.6 Property of Deformation and Motion Tensors Under Reference Frame Transformation 4.7 Objective Rates 4.7.1 Some Objective Rates 4.7.2 Physical Meaning of the Jaumann Stress Rate 4.8 Finite Elasticity 4.8.1 The Cauchy Elasticity 4.8.2 Hyperelasticity 4.8.3 Isotropic Hyperelastic Materials 4.8.4 Applications of Isotropic Hyperelasticity 4.9 Inﬁnitesimal Theory of Elasticity 4.9.1 Constitutive Equation 4.9.2 Homogeneous Deformations 4.9.3 Boundary-Value Problems 4.10 Hypoelasticity References Problems

141 141 142 145 145 146 148

Part II 5

vii

150 150 151 163 164 166 169 169 172 174 175 177 181 185 193 193 195 197 197 200 200

Continuum Theory of Plasticity

Fundamentals of Continuum Plasticity 5.1 Introduction

© 2005 by Chapman & Hall/CRC Press

205 205

viii

6

7

Contents 5.2

Some Basic Mechanical Tests 5.2.1 The Uniaxial Tension Test 5.2.2 The Uniaxial Compression Test 5.2.3 The Torsion Test 5.2.4 Strain Rate, Temperature, and Creep 5.3 Modeling the Stress–Strain Curve 5.4 The Effects of Hydrostatic Pressure 5.5 Torsion Test in the Large Strain Range 5.5.1 Introduction 5.5.2 Experimental Program and Procedures 5.5.3 Experimental Results and Discussions 5.5.4 Determination of Shear Stress–Strain Curve References Problems

209 209 216 219 225 231 234 237 237 241 246 256 260 263

The Flow Theory of Plasticity 6.1 Introduction 6.2 The Concept of Yield Criterion 6.2.1 Mathematical Expressions of Yield Surface 6.2.2 Geometrical Representation of Yield Surface in the Principal Stress Space 6.3 The Flow Rule 6.4 The Elastic-Perfectly Plastic Material 6.5 Strain-Hardening 6.5.1 Drucker’s Postulate 6.5.2 The Isotropic-Hardening Rule 6.5.3 The Kinematic-Hardening Rule 6.5.4 General Form of Subsequent Yield Function and Its Flow Rule 6.6 The Return-Mapping Algorithm 6.7 Combined Axial–Torsion of Strain-Hardening Materials 6.8 Flow Theory in the Strain Space 6.9 Remarks References Problems

265 265 265 269

Advances in Plasticity 7.1 Introduction 7.2 Experimenal Determination of Yield Surfaces 7.2.1 Factors Affecting the Determination of Yield Surface 7.2.2 A Summary of Experiments Related to the Determination of Yield Surfaces 7.2.3 Yield Surface Versus Loading Surface 7.2.4 Yield Surface at Elevated Temperature 7.3 The Direction of the Plastic Strain Increment 7.4 Multisurface Models of Flow Plasticity

323 323 324

© 2005 by Chapman & Hall/CRC Press

271 274 276 286 287 290 296 301 306 308 314 316 317 318

325 328 333 335 336 340

Contents 7.4.1 The Mroz Kinematic-Hardening Model 7.4.2 The Two-Surface Model of Dafalias and Popov 7.5 The Plastic Strain Trajectory Approach 7.5.1 The Theory of Ilyushin 7.5.2 The Endochronic Theory of Plasticity 7.6 Finite Plastic Deformation 7.6.1 The Stress and Strain Measures 7.6.2 The Decomposition of Strain and Strain Rate 7.6.3 The Objective Rates 7.6.4 A Theory of Finite Elastic–Plastic Deformation 7.6.5 A Study of Simple Shear Using Rigid-Plastic Equations with Linear Kinematic Hardening 7.6.6 The Yield Criterion for Finite Plasticity References Problems 8

9

Internal Variable Theory of Thermo-Mechanical Behaviors and Endochronic Theory of Plasticity 8.1 Introduction 8.2 Concepts and Terminologies of Thermodynamics 8.2.1 The First Law of Thermodynamics 8.2.2 State Variables, State Functions, and the Second Law of Thermodynamics 8.3 Thermodynamics of Internal State Variables 8.3.1 Irreversible Systems 8.3.2 The Clausius–Duhem Inequality 8.3.3 The Helmholtz Formulation of Thermo-Mechanical Behavior 8.3.4 The Gibbs Formulation of Thermo-Mechanical Behavior 8.4 The Endochronic Theory of Plasticity 8.4.1 The Concepts of the Endochronic Theory 8.4.2 The Simple Endochronic Theory of Plasticity 8.4.3 The Improved Endochronic Theory of Plasticity 8.4.4 Derivation of the Flow Theory of Plasticity from Endochronic Theory 8.4.5 Applications of the Endochronic Theory to Metals 8.4.6 The Endochronic Theory of Viscoplasticity References Problems Topics in Endochronic Plasticity 9.1 Introduction 9.2 An Endochronic Theory of Anisotropic Plasticity 9.2.1 An Endochronic Theory Accounting for Deformation Induced Anisotropy 9.2.2 An Endochronic Theory for Anisotropic Sheet Metals

© 2005 by Chapman & Hall/CRC Press

ix 340 344 351 351 356 357 358 358 364 368 374 384 393 397 399 399 399 399 400 403 403 405 406 408 410 410 412 421 425 427 441 450 452 455 455 455 455 461

x

Contents 9.3

10

Endochronic Plasticity in the Finite Strain Range 9.3.1 Corotational Integrals 9.3.2 Endochronic Equations for Finite Plastic Deformation 9.3.3 Application to a Rigid-Plastic Thin-Walled Tube Under Torsion 9.4 An Endochronic Theory for Porous and Granular Materials 9.4.1 The Endochronic Equations 9.4.2 Application to Concrete 9.4.3 Application to Sand 9.4.4 Application to Porous Aluminum 9.5 An Endochronic Formulation of a Plastically Deformed Damaged Continuum 9.5.1 Introduction 9.5.2 The Anisotropic Damage Tensor 9.5.3 Gross Stress, Net Stress, and Effective Stress 9.5.4 An Internal State Variables Theory 9.5.5 Plasticity and Damage 9.5.6 The Constitutive Equations and Constraints 9.5.7 A Brief Summary of Wu and Nanakorn’s Endochronic CDM 9.5.8 Application 9.5.9 Concluding Remarks References Problems

468 469

Anisotropic Plasticity for Sheet Metals 10.1 Introduction 10.2 Standard Tests for Sheet Metal 10.2.1 The Uniaxial Tension Test 10.2.2 Equibiaxial Tension Test 10.2.3 Hydraulic Bulge Test 10.2.4 Through-Thickness Compression Test 10.2.5 Plane-Strain Compression Test 10.2.6 Simple Shear Test 10.3 Experimental Yield Surface for Sheet Metal 10.4 Hill’s Anisotropic Theory of Plasticity 10.4.1 The Quadratic Yield Criterion 10.4.2 The Flow Rule and the R-Ratio 10.4.3 The Equivalent Stress and Equivalent Strain 10.4.4 The Anomalous Behavior 10.5 Nonquadratic Yield Functions 10.6 Anisotropic Plasticity Using Combined Isotropic–Kinematic Hardening 10.6.1 Introduction

543 543 545 545 545 545 545 546 546 546 548 548 550

© 2005 by Chapman & Hall/CRC Press

474 476 487 490 500 502 503 506 506 507 512 516 521 523 526 530 535 537 541

552 553 555 558 558

Contents 10.6.2 The Anisotropic Theory Using Combined Isotropic–Kinematic Hardening 10.6.3 Results and Discussion 10.6.4 Summary and Conclusion References Problems 11

12

Description of Anisotropic Material Behavior Using Curvilinear Coordinates 11.1 Convected Coordinate System and Convected Material Element 11.2 Curvilinear Coordinates and Base Vectors 11.3 Tensors and Special Tensors 11.4 Multiplication of Vectors 11.5 Physical Components of a Vector 11.6 Differentiation of a Tensor with Respect to the Space Coordinates 11.6.1 Derivative of a Scalar 11.6.2 Derivatives of a Vector 11.6.3 Derivatives of a Tensor 11.7 Strain Tensor 11.8 Strain–Displacement Relations 11.9 Stress Vector and Stress Tensor 11.10 Physical Components of the Stress Tensor 11.11 Other Stress Tensors and the Cartesian Stress Components 11.12 Stress Rate and Strain Rate 11.13 Further Discussion of Stress Rate 11.14 A Theory of Plasticity for Anisotropic Metals 11.14.1 The Yield Function 11.14.2 The Flow Rule 11.14.3 The Strain Hardening 11.14.4 Elastic Constitutive Equations References Problems Combined Axial–Torsion of Thin-Walled Tubes 12.1 Introduction 12.2 Convected Coordinates in the Combined Axial–Torsion of a Thin-Walled Tube 12.3 The Yield Function 12.3.1 The Mises Yield Criterion 12.3.2 A Yield Criterion Proposed by Wu 12.4 Flow Rule and Strain Hardening 12.5 Elastic Constitutive Equations 12.6 Algorithm for Computation 12.7 Nonlinear Kinematic Hardening

© 2005 by Chapman & Hall/CRC Press

xi

560 566 572 575 577 579 579 580 584 590 591 592 593 593 594 599 603 606 609 610 612 617 619 621 628 628 629 630 631 633 633 634 637 637 638 642 646 647 649

xii

Contents 12.8 Description of Yield Surface with Various Preloading Paths 12.8.1 Path (1) — Axial Tension 12.8.2 Path (2) — Torsion 12.8.3 Path (3) — Proportional Loading 12.8.4 Tor–Ten Path (4) 12.8.5 Tor–Ten Path (5) 12.8.6 Tor–Ten Path with Constant Shear Strain 12.9 A Stress Path of Tension-Unloading Followed by Torsion 12.10 Summary and Discussion References Problems

Answers and Hints to Selected Problems

© 2005 by Chapman & Hall/CRC Press

649 652 656 660 660 662 664 665 668 669 670 671

Preface One of the aims of this book is to bring the subjects of continuum mechanics and plasticity together so that students will learn about the principles of continuum mechanics and how they are applied to the formulation of plasticity theory. Continuum Mechanics and Plasticity were traditionally two separate courses, and students had to make extra efforts to relate the two subjects in order to read the modern literature on plasticity. Another aim of this book is to include sufﬁcient background material about the experimental aspect of plasticity. Experiments are presented and discussed with reference to the veriﬁcation of theories. With knowledge of the experiments, the reader can make better judgments when realistic constitutive equations of plasticity are used. A third aim is to include anisotropic plasticity in this book. This important topic has not been fully discussed in most plasticity books on engineering mechanics. The ﬁnal aim of the book is to incorporate research results obtained by me and my coworkers related to the endochronic theory of plasticity, so that these results can be systematically presented and better understood by readers. Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (continuum) approach is still the practical approach for use in the simulation of engineering problems. Most current computations use a theory of plasticity for isotropic material and work with the Cauchy stress. However, material anisotropy has long existed in real structural components and machine parts. Its effect has mostly been neglected for the sake of computational simplicity, but material anisotropy does play a signiﬁcant role in the manufacturing process. A realistic description of material anisotropy may help reduce scraps in the manufacturing processes and reduce the amount of energy wasted. Also, components may be designed to possess certain predesigned anisotropy to enhance their performance. This book addresses the issue of material anisotropy by using the contravariant true stress that is deﬁned based on convected coordinates. A material element should be followed during anisotropic plastic deformation, where a square material element will no longer be square, and convected (curvilinear) coordinates should be used together with general tensors. The popular Cauchy stress is not useful in deﬁning the yield criterion, because it is deﬁned with respect to a rectangular Cartesian element. Even though recent works in computational mechanics have mostly been based on the Cartesian coordinate system, an understanding of the curvilinear coordinate system by computational mechanists and engineers will help develop computational algorithms suitable to addressing the issue of material anisotropy. Most books xiii

© 2005 by Chapman & Hall/CRC Press

xiv

Preface

that cover general tensors in curvilinear coordinates were published in the early 1960s and treat mainly elastic deformations. In this book, I devote a signiﬁcant number of pages to discussing a modern theory of plasticity using curvilinear coordinates. Recently published books address mainly computational methods and algorithms, neglecting the signiﬁcance of experimental study and material anisotropy. Their purpose is to discuss efﬁcient and stable methods and algorithms for analysis and design. In doing so, simple constitutive models are used for computational simplicity. Sometimes, unrealistic conditions, such as a nonsmooth yield function, have been discussed at length. A nonsmooth yield function has never been experimentally observed. Owing to tremendous advances in computer technologies and methods, computational power doubles and redoubles in a short time. Consequently, there will shortly be a demand for reﬁnements of constitutive models of plasticity. What is acceptable today will no longer be acceptable in the near future. At that time, an acceptable model will, among other things, be able to account for material anisotropy and produce results that compare well with experimental data. This book will help readers in meeting this challenge. I taught the subjects of continuum mechanics, elasticity, and plasticity in four separate semester-long courses at the University of Iowa from 1970 to 1986. During this period, the contents of these courses were constantly updated. Since 1987, I have been teaching a two-course series to replace these four courses. This new series essentially narrows down the coverage of continuum mechanics to solids (in the sense that no special treatment of ﬂuids and gases is included). However, it provides a more systematic and comprehensive coverage of the subject of the mechanics of solids. This book grew out of my lecture notes for the two-course series. There were three reasons for this change at the time, and these are still valid today. (1) A modern trend: Owing to recent advances in plasticity, the methods of continuum mechanics have been used to develop new theories of plasticity or to reformulate the existing theories. Therefore, in modern literature, continuum mechanics is essential to the understanding of plasticity. (2) Reduction of the number of courses offered: The original four courses have been reduced to two. Owing to budget constraints, it has been necessary for many engineering colleges, including the College of Engineering at the University of Iowa, to reduce the number of courses offered to students. (3) Suitability for students of computational solid mechanics: Owing to advances in computing technologies and methods, students of computational solid mechanics must use modern continuum mechanics and plasticity to obtain realistic numerical solutions to their engineering problems. These students need not only courses in continuum mechanics and plasticity but also courses that are oriented toward computation and data handling. The students are limited in terms of the number of courses that they can take but still need to learn the subjects well. The two-course series based on this book ﬁts the needs of this student group to integrate subject matter by the most efﬁcient means possible.

© 2005 by Chapman & Hall/CRC Press

Preface

xv

The book is divided into two parts: Part I — Fundamentals of Continuum Mechanics and Part II — Continuum Theory of Plasticity. Part I (Chapters 1 to 4) is suitable for use as a textbook at the ﬁrst-year graduate level for aerospace engineering, civil engineering, engineering mechanics, materials engineering, and mechanical engineering students. It is also suitable for use by advanced undergraduate students of applied mathematics. A second course may be taught to advanced graduate students from selected topics from Part II (Chapters 5 to 12). Since the book contains up-to-date materials, it may also be used by researchers and engineers as a reference book. The chapters are divided into sections and subsections. Technical terms are written in italic font when they ﬁrst appear. Examples are given within the text when further clariﬁcation is called for, and exercise problems are given at the end of each chapter. Mathematical fundamentals and Cartesian tensors are covered in Chapter 1; the concepts of the stress vector, the stress tensor, and stress invariants are discussed in Chapter 2; Chapter 3 discusses the kinematics of deformation; and Chapter 4 discusses the conservation laws, the constitutive equations, and elasticity. In this chapter, examples related to different stress measures are given. I have written Chapter 5 — Fundamentals of Continuum Plasticity from the viewpoint of an experimentalist with constitutive modeling in mind. The reader will acquire a general knowledge about different types of mechanical tests and the resulting material behavior in the small and large strain ranges. Potential sources of data uncertainty have been pointed out and discussed. In particular, I have discussed the hydrostatic pressure effect of yield stress and the assumption of plastic incompressibility. The reader will learn the classical ﬂow theory of plasticity in Chapter 6. I discuss recent advances in plasticity in Chapter 7, both experimentally and theoretically. In particular, I include ﬁnite plastic deformations with various objective rates and a discussion of yield surfaces determined using different stress measures. The fundamentals of endochronic theory are given in Chapter 8 and, in Chapter 9, I present topics of endochronic theory, which include anisotropic plasticity, ﬁnite strain, porous and granular materials, and a plastically deformed damaged continuum. Anisotropic plasticity is discussed further in Chapters 10 to 12. In Chapter 10, the discussion is of sheet metals. In Chapter 11, ﬁrst the fundamentals of the curvilinear coordinate system and general tensors and then the stress and strain with reference to the convected material element are discussed. Next different stress tensors and the stress rates are discussed. At the end of the chapter, a general theory of anisotropic plasticity is presented. Finally, in Chapter 12, the theory of Chapter 11 is applied to investigate the path-dependent evolution of the yield surface in the case of the combined axial-torsion of thin-walled tubes. I learned plasticity from the late Professor Aris Phillips of Yale University, who is well known for his life-time effort to determine yield surfaces. I then had the honor and privilege of working with Professor Kirk C. Valanis, who was a senior professor and departmental chair at Iowa during the 1970s. Professor Valanis is well known for his endochronic theory of plasticity, which

© 2005 by Chapman & Hall/CRC Press

xvi

Preface

at the time advocated a theory of plasticity without a yield surface. The years of working and having discussions with Kirk were most stimulating and inspiring, and he turned me into a disciple of his theory. As a result, I have spent most of my academic life in experimentally verifying and further developing the endochronic theory. During the same time, I have continued Professor Phillips’s efforts in the experimental determination of yield surface, and extended them into the large strain range. There is no doubt that yield surfaces can be experimentally determined, with some data scatter. It may be more appropriate to talk about a yield band with certain amounts of uncertainty than of a yield locus. The direction of plastic strain increment is, therefore, also associated with certain amounts of uncertainty. Kirk has since shown that yield surface can be derived from the endochronic theory in a limit case. I now view yield surface as a means of getting to an approximate solution of the problem at hand. Indeed, in many cases, a theory without a yield surface can have advantages in computation since all equations are continuous. I am indebted to the late Dr. Owen Richmond and to Dr. Paul T. Wang of Alcoa Laboratories for their continuing support of my research. The research support from the NSF, NASA, and the U.S. Army is also appreciated. I wish to express my sincere gratitude to the University of Iowa for the Career Development Award for the fall semester of the academic year 2001–2002. The award enabled me to plan for the book and start the initial part of my writing. My appreciation also extends to Professor David Y. Gao for his invitation to write this book and to Mr. Robert B. Stern, acquisitions editor and executive editor of CRC Press, for his assistance in publishing this book. Finally, I am thankful to my wife Yumi, whose love, encouragement, and patience enabled me to complete the writing of this book. Han-Chin Wu Iowa City, April 2004

© 2005 by Chapman & Hall/CRC Press

Author Professor Han-Chin Wu received his B.S. degree in civil engineering from National Taiwan University, his M.S. degree in structural engineering from the University of Rhode Island, and his M.S. and Ph.D. degrees in the mechanics of solids from Yale University. He has been teaching at the University of Iowa since 1970 and has supervised 19 Ph.D. students to completion. Dr. Wu is a professor in the Department of Civil and Environmental Engineering. He is also a professor of Mechanical Engineering and a fellow of American Society of Mechanical Engineers. His research interest is in the mechanical behavior (plastic ﬂow, damage, creep, fracture, and fatigue) of metals and porous and granular materials such as porous aluminum, concretes, ice, and soils. His methods are both experimental and theoretical in an effort at constitutive modeling. He is the author of 70 journal publications and more than 100 conference papers and research reports, and he has a patent on an axial– torsional extensometer for large strain testing.

xvii

© 2005 by Chapman & Hall/CRC Press

Part I

Fundamentals of Continuum Mechanics Continuum mechanics is a branch of mechanics concerned with stresses in solids, ﬂuids, and gas and the deformation or motion of these materials. A major assumption is that mass is continuous in a continuous medium and that the density can be deﬁned.

© 2005 by Chapman & Hall/CRC Press

1 Cartesian Tensors

1.1

Introduction

In this chapter, we discuss the basics of Cartesian tensors with the purpose of preparing the reader for subsequent chapters on continuum mechanics and plasticity. Curvilinear coordinates and general tensors as well as more advanced topics are discussed in Chapters 11 and 12. First, we discuss the notations in detail: both symbolic and index notations are used in this book. The symbolic notations simplify the equations and will help the reader in understanding the structure of the equations as the subscripts may be confusing. However, when a set of coordinate systems has been assigned, we utilize the index notation. We first discuss the tensor algebra, and then the differentiation and integration of tensors, which are standard materials. Some references [1–5] are given at the end of the chapter for additional reading.

1.1.1

Notations

In the symbolic notation, a vector is expressed by a bold-faced lowercase letter, say a, or by notations such as a, a, a, etc.; a tensor is expressed by a bold-faced ˜ such as A, A, A , etc. In the index notation, capital letter, say A, or by notations ˜ the components of a vector (the meaning of components will be discussed in Section 1.2.1) are denoted by ai , and the components of a second-rank tensor (discussed in Section 1.3.1) are denoted by Aij , or Tijk for a third-rank tensor. We note that a second-rank tensor has two subscripts, a third-rank tensor has three subscripts, and an nth-rank tensor has n subscripts. Summation and range conventions are used in the index notation. In the summation convention, a repeated index means summation of the term over the range of the index. For example, Akk = A11 + A22 + A33 , if the range of the index is from 1 to 3. On the other hand, if the range of the index is from 1 to n, then Akk = A11 + A22 + · · · + Ann , a sum of n terms. We note that the underscored n does not imply summation, and the index should not repeat more than once. The notation Akkk , for instance, is not deﬁned. The repeated index 3

© 2005 by Chapman & Hall/CRC Press

4

Continuum Mechanics and Plasticity

k is called a dummy index because it can be replaced by another index with no difference in its outcome. For example, Akk = Aii = Ajj = A11 + A22 + A33 . The range convention applies when there is a free (not repeated) index in a term. The free index takes a value of 1, 2, or 3 for a three-dimensional space. Equation yi = Cij xj is actually a set of three equations, and i is the free index. You may apply the range convention as follows: For i = 1,

y1 = C1j xj = C11 x1 + C12 x2 + C13 x3

For i = 2,

y2 = C2j xj = C21 x1 + C22 x2 + C23 x3

For i = 3,

y3 = C3j xj = C31 x1 + C32 x2 + C33 x3

(1.1)

Note that the summation convention has been applied in the last equality of each of the above equations.

1.1.2

Cartesian Coordinate System

We use (x1 , x2 , x3 ) instead of (x, y, z) to denote the axes of the Cartesian coordinate system. Sometimes, the coordinate axes may simply be denoted by 1, 2, and 3 in a ﬁgure. Using the index notation, the axes are xi . Throughout this book, the right-handed coordinate system will be used.

1.1.3

Special Tensors

There are two special tensors, δij and eijk , which are often used to simplify mathematical expressions. Kronecker’s delta δij is deﬁned as δij = 1

when i = j

=0

when i = j

(1.2)

Examples are δ11 = δ22 = δ33 = 1 and δ12 = δ21 = δ13 = δ23 = 0, etc. Using the summation convention, we ﬁnd δii = δ11 + δ22 + δ33 = 3. In the symbolic notation, Kronecker’s delta is a unit tensor 1, or it may be written as δ. A useful feature of Kronecker’s delta is its substitution property. We can then write δij aikp = ajkp , replacing i by j in the expression aikp . The permutation symbol eijk is also known as the alternating tensor, and it is deﬁned by

eijk

+1 = 0 −1

even permutation of 1, 2, 3 two or more subscripts are the same odd permutation of 1, 2, 3

(1.3)

Examples are e123 = e231 = e312 = 1, e321 = e132 = e213 = −1, and e112 = e133 = e111 = 0, etc.

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

1.2 1.2.1

5

Vectors Base Vectors and Components

In three-dimensional Euclidean space, the base vectors are e1 , e2 , and e3 . The base vectors are unit vectors in the Cartesian coordinate system and are not necessarily unit vectors in the curvilinear coordinate system (curvilinear coordinates are discussed in Chapter 11). In the Cartesian system, the base vectors are mutually perpendicular to each other. A vector a may be expressed as a = ap ep = a1 e1 + a2 e2 + a3 e3

(1.4)

where ap are the components of a relative to the basis ep . 1.2.2

Vector Addition and Multiplication

Vectors a and b may be added as follows: a + b = ap ep + bp ep = (ap + bp )ep

(1.5)

There are two kinds of multiplication, the scalar product and the vector product. The scalar product, also known as the dot product, of two base vectors ei and ej is ei · ej = δij

(1.6)

Examples are, when i = 1 and j = 2, e1 · e2 = 0, that is, e1 is perpendicular to e2 ; when i = 1 and j = 3, e1 · e3 = 0, which means that e1 is perpendicular to e3 . Generally, ei is perpendicular to ej for any permutation of i and j. The scalar product of vectors a and b is expressed by a · b = (ap ep ) · (bq eq ) = ap bq ep · eq = ap bq δpq = ap bp

(1.7)

The outcome of the scalar multiplication is also a scalar. Using this expression, the norm or the magnitude of vector a is given by |a| = [a · a]1/2 = [ap ap ]1/2

(1.8)

Thus, by use of (1.8), the norm of ei is one. The vector product is also known as the cross product. The outcome of a cross product is a vector. The cross products between Cartesian base vectors are e2 × e3 = e1 , e3 × e1 = e2 , e1 × e2 = e3 , which may be summarized by the following expression: ei × ej = ±eijp ep

© 2005 by Chapman & Hall/CRC Press

(1.9)

6

Continuum Mechanics and Plasticity

where the “+” sign applies for the right-handed coordinate system and the “−” sign applies for the left-handed coordinate system. Since the righthanded coordinate system will be used throughout this book, we will disregard the “−” sign from now on. By use of this notation, the cross product between vectors a and b becomes a × b = (ap ep ) × (bq eq ) = ap bq ep × eq = epqr ap bq er

(1.10)

Using the dot product, the components of a vector may be found as a · ei = ap ep · ei = ap δpi = ai

(1.11)

Therefore, vector a may be expressed as a = (a · ep )ep

(1.12)

The scalar triple product of vectors a, b, and c is a · (b × c) = ai ei · epqr bp cq er = epqr ai bp cq δir = epqr ar bp cq = epqr ap bq cr

(1.13)

The last expression of (1.13) was obtained by permutation of indices. The scalar triple product represents the volume of an element formed by vectors a, b, and c as its sides.

1.2.3

The e–δ Identity

The following identity is known as the e–δ identity. This identity has been frequently applied to provide simpliﬁed expressions in vector calculus. The identity is eijk eiqr = δjq δkr − δjr δkq

δ = jq δkq

δjr δkr

(1.14)

Note that i is summed. EXAMPLE 1.1

Prove the e–δ identity.

Proof We ﬁrst establish the identity

epqs emnr

© 2005 by Chapman & Hall/CRC Press

δmp = δnp δrp

δmq δnq δrq

δms δns δrs

(a)

Cartesian Tensors

7

To this end, we let T11 det T = T21 T31

T13 T23 T33

T12 T22 T32

(b)

Since an interchange of two rows in the determinant causes a sign change, we have Tm1 emnr det T = Tn1 Tr1

Tm3 Tn3 Tr3

Tm2 Tn2 Tr2

(c)

An interchange of columns causes a sign change too, and we also write T1p epqs det T = T2p T3p

T1s T2s T3s

T1q T2q T3q

(d)

For an arbitrary row and column interchange sequence, we can, therefore, write

emnr epqs

Tmp det T = Tnp Trp

Tmq Tnq Trq

Tms Tns Trs

(e)

When Tij = δij and det T = 1, the above equation is reduced to

emnr epqs

δmp = δnp δrp

δmq δnq δrq

δms δns δrs

(f)

which is the same as (a). The e–δ identity may then be obtained by setting m = p in (f). Expanding the resulting determinant on the right-hand side of the equation, this leads to emnr emqs = δmm (δnq δrs − δrq δns )− δmq (δnm δrs − δrm δns )+ δms (δnm δrq − δrm δnq ) = δmm (δnq δrs − δrq δns ) − 2(δnq δrs − δrq δns ) δ δ = δnq δrs − δrq δns = nq ns δrq δrs which is the e–δ identity given by (1.14).

© 2005 by Chapman & Hall/CRC Press

(g)

8

Continuum Mechanics and Plasticity

EXAMPLE 1.2 The e–δ identity may be applied to prove other identities. An example is to prove the following identity:

a × (b × c) = b(a · c) − c(a · b)

Proof LHS = ai ei × (bj ej × ck ek ) = ai ei × (erjk bj ck er ) = erjk ai bj ck (ei × er ) = erjk esir ai bj ck es = erjk ersi ai bj ck es = (δjs δki − δji δks )ai bj ck es = δjs δki ai bj ck es − δji δks ai bj ck es = ai bj ci ej − ai bi ck ek = (ai ci )bj ej − ck ek (ai bi ) = RHS Similarly, the following identities may be proven: a · (b × c) = (a × b) · c (a × b) · (c × d) = (a · c)(b · d) − (a · d)(b · c) (a × b) × (c × d) = b[a · (c × d)] − a[b · (c × d)]

1.3

The Transformation of Axes

Consider the rectangular Cartesian coordinate system x1 , x2 , and x3 shown in Figure 1.1. If we rotate the coordinate system through some angle about its origin O, the new coordinate axes become x1 , x2 , and x3 . The direction cosines between xi and xj are Qij = cos(xi , xj )

(1.15)

where the ﬁrst subscript denotes the unprimed axes and the second subscript the primed axes. In general, Qij = Qji , e.g., Q23 = Q32 ,

or

cos(x2 , x3 ) = cos(x3 , x2 ).

In the matrix form, we write Qij as

Q11 [Q] = Q21 Q31

© 2005 by Chapman & Hall/CRC Press

Q12 Q22 Q32

Q13 Q23 Q33

(1.16)

Cartesian Tensors

9 x3

x′3 x′2 A

e3 e′3

e′2 x2

e2

O

e⬘1 e1 x′1 x1 FIGURE 1.1 Transformation of coordinate systems.

We now discuss the properties of the transformation matrix [Q]. From vector −→ analysis and referring to Figure 1.1, the unit vector OA is expressed as −→ −→ −→ −→ OA = cos(x1 , OA)e1 + cos(x2 , OA)e2 + cos(x3 , OA)e3

(1.17)

−→ If we take OA along the x1 direction, and denote the vector by e 1 , then (1.17) becomes e 1 = cos(x1 , x1 )e1 + cos(x2 , x1 )e2 + cos(x3 , x1 )e3 = Q11 e1 + Q21 e2 + Q31 e3 = Qj1 ej

(1.18)

Equation (1.18) shows that Qj1 are direction cosines for the unit vector e 1 . −→ Since the magnitude of OA is one, we write 2 2 2 Q11 + Q21 + Q31 =1

or

Qi1 Qi1 = 1

(1.19)

−→ Similarly, if we take OA along the x2 direction and denote the vector by e 2 , we obtain 2 2 2 Q12 + Q22 + Q32 =1

© 2005 by Chapman & Hall/CRC Press

or

Qi2 Qi2 = 1

(1.20)

10

Continuum Mechanics and Plasticity

−→ Again, if we take OA along the x3 direction and denote the vector by e 3 , we get 2 2 2 + Q23 + Q33 =1 Q13

or

Qi3 Qi3 = 1

(1.21)

A general form of equation (1.18) is e i = Qji ej

(1.22)

Since e i and e j (i = j) are perpendicular to each other, their dot products are zero. Therefore, from (1.22), e i · e j = (Q1i e1 + Q2i e2 + Q3i e3 ) · (Q1j e1 + Q2j e2 + Q3j e3 ) = Q1i Q1j + Q2i Q2j + Q3i Q3j = 0

(1.23)

and we obtain Qki Qkj = 0

i = j

for

(1.24)

Summarizing (1.19)–(1.21) and (1.24), we write Qki Qkj = δij

(1.25)

When i = j, (1.25) reduces to (1.19)–(1.21); and when i = j, (1.25) reduces to (1.24). In the matrix notation, we then have [Qik ]T [Qkj ] = [δij ]

or simply

[Q]T [Q] = [1]

(1.26)

Note that [Qik ]T = [Qki ] is the transpose of matrix [Qik ]. When performing matrix multiplication, the summation convention is used adjacently, that is, a dummy index is used for two adjacent subscripts in matrix multiplication. Equation (1.26) is an important relationship. The matrix [Q] is orthogonal, which will be discussed further in Section 1.6.1. In a similar manner, we can show that Qik Qjk = δij

or

[Q][Q]T = [1]

(1.27)

−→ This is accomplished by taking unit vector OA along x1 , x2 , and x3 , respectively, and ﬁnding projections of ei on the xi axes. Thus, ei = Qi1 e 1 + Qi2 e 2 + Qi3 e 3 = Qij e j

(1.28)

and the magnitude of the vector is Qik Qik = 1

© 2005 by Chapman & Hall/CRC Press

for

i = 1, 2, 3

(1.29)

Cartesian Tensors

11

If we consider the dot products between ei and ej , we obtain Qik Qjk = 0

i = j

for

(1.30)

The above two equations lead to (1.27). We rewrite (1.22) and (1.28) here to emphasize their importance in the transformation of axes: e i = Qji ej

(1.22)

ei = Qij e j

(1.28)

and

These are equations relating the base vectors of the primed and unprimed coordinate systems. In (1.22), QijT transforms a unit vector ei into the unit vector e i and, in (1.28), Qij transforms the unit vector e i back into ei . The direction cosines Qki may also be obtained from ek · e i = ek · Qji ej = δkj Qji = Qki

(1.29)

The transformation formula for vector a is a = a i e i = aj ej = aj Qji e i

or

a i = Qji aj

(1.30)

or, in the matrix form, [a ] = [Q]T [a]

(1.31)

The inverse relation of (1.31) is obtained by writing a = aj ej = a i e i = a i Qji ej

or

ai = Qij a j

(1.32)

or, in the matrix form, [a] = [Q][a ]

(1.33)

Note that the same Qij is used in both relations (1.31) and (1.33). Finally, we note that the scalar product of vectors a and b is a · b = a i b i = Qji aj Qki bk = δjk aj bk = aj bj = ai bi

(1.34)

We see from (1.34) that the value of a · b is independent of the coordinate system to which the components are referred. A quantity with such a property is called an invariant.

© 2005 by Chapman & Hall/CRC Press

12

1.4

Continuum Mechanics and Plasticity

The Dyadic Product (The Tensor Product)

Some physical quantities require the speciﬁcation of two vectors for their description. Quantities of this kind can be described by a dyadic product. The dyadic product of two vectors u and v is written as u ⊗ v. It has the associative and distributive properties given by (αu) ⊗ v = u ⊗ (αv) = α(u ⊗ v) u ⊗ (v + w) = u ⊗ v + u ⊗ w,

(v + w) ⊗ u = v ⊗ u + w ⊗ u

(1.35)

where α is a scalar. In terms of the components of u and v, u ⊗ v may be written as u ⊗ v = (ui ei ) ⊗ (vj ej ) = ui vj ei ⊗ ej = u1 v1 e1 ⊗ e1 + u1 v2 e1 ⊗ e2 + u1 v3 e1 ⊗ e3 + u 2 v1 e2 ⊗ e 1 + u 2 v2 e2 ⊗ e 2 + u 2 v3 e2 ⊗ e 3 + u 3 v1 e3 ⊗ e 1 + u 3 v2 e3 ⊗ e 2 + u 3 v3 e3 ⊗ e 3

(1.36)

The components of u ⊗ v are ui vj , which can be displayed in a matrix:

u 1 v1 [u ⊗ v] = u2 v1 u3 v1

u1 v2 u2 v2 u3 v2

u1 v3 u2 v3 u3 v3

(1.37)

The dyadic products ei ⊗ ej of the base vectors ei are called unit dyads. Thus, the dyadic product u ⊗ v is expressed in (1.36) in terms of its components ui vj and its bases ei ⊗ ej . The form of (1.36) is independent of the choice of the coordinate system. Using (1.22, 1.27, 1.30), we obtain u i vj e i ⊗ e j = Qpi up Qqj vq Qri er ⊗ (Qsj es ) = Qpi Qri Qqj Qsj up vq er ⊗ es = δpr δqs up vq er ⊗ es = ur vs er ⊗ es = ui vj ei ⊗ ej

(1.38)

In general, the commutative law is not valid, that is, u ⊗ v = v ⊗ u. An additional property of a dyadic product is that it forms an inner product with a vector. We may take the following relations as deﬁnitions: (u ⊗ v) · w = u(v · w),

u · (v ⊗ w) = (u · v)w

(1.39)

u · v ⊗ w = (u · v)w

(1.40)

These relations may also be written as u ⊗ v · w = u(v · w),

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

13

since there is no possibility of ambiguity. We see in (1.39) and (1.40) that an inner product of a dyadic product with a vector yields another vector. The concept of a dyadic product can be extended to products of three or more vectors. Thus, the product of three vectors u, v, and w is a triad and is written u ⊗ v ⊗ w. Similarly, we can deﬁne tetrads or higher-order polyads. The triad u ⊗ v ⊗ w in its component form is written as ui vj wk ei ⊗ ej ⊗ ek .

1.5 1.5.1

Cartesian Tensors General Properties

We deﬁne a second-rank (order) Cartesian tensor as a linear combination of dyadic products. Since, from (1.36), a dyadic product is itself a linear combination of unit dyads, a second-rank Cartesian tensor T can be expressed as a linear combination of unit dyads. This deﬁnition of a Cartesian tensor is equivalent to deﬁning the tensor as a linear transformation that transforms a vector into another vector. We see from (1.39) that u ⊗ v transforms a vector into another vector and, from (1.35), that it obeys the associative and distributive properties of a linear transformation. Therefore, u ⊗ v is a tensor. In the component form, tensor T is written as T = Tij ei ⊗ ej = T11 e1 ⊗ e2 + T12 e1 ⊗ e2 + T13 e1 ⊗ e3 + T21 e2 ⊗ e1 + · · · (1.41) The coefﬁcients Tij are called the components of T. We will denote tensor components by the same letter that we use to denote the tensor itself and remark that a tensor exists independently of any coordinate system. Its components can only be speciﬁed after a coordinate system has been chosen, and the values of the components depend on the choice of the coordinate system. If, in a new coordinate system with base vectors e i , tensor T has components Tij , then from (1.41)

T = Tij ei ⊗ ej = Tpq ep ⊗ e q

(1.42)

Tij ei ⊗ ej = Tij Qip Qjq e p ⊗ e q

(1.43)

But, by use of (1.28),

Therefore, by equating the above two equations, their coefﬁcients are related by

Tpq = Qip Qjq Tij

© 2005 by Chapman & Hall/CRC Press

or

T Tpq = Qpi Tij Qjq

(1.44)

14

Continuum Mechanics and Plasticity

This is the transformation formula for components of second-rank tensors. Equation (1.44) may also be considered as an alternative deﬁnition of a secondrank tensor. In order to identify a second-rank tensor as such, we may show that its components transform according to (1.44) from one coordinate system, xi , to another, xi . The nine components of Tij may be displayed in a 3×3 square matrix [T], so that the above equation may be written in a matrix equation as [T ] = [Q]T [T][Q].

(1.45)

The matrix form is often convenient for algebraic manipulation. We now extend the relation (1.41) to express a Cartesian tensor of rank (order) n in terms of components as T = Tij···m ei ⊗ ej ⊗ · · · ⊗ em

(1.46)

Note that the components Tij...m have n indices and the tensor product has n factors. The components of this nth-rank tensor transform according to the rule

Tpq...t = Qip Qjq · · · Qmt Tij...m

(1.47)

From this more general viewpoint, a scalar can be interpreted as a tensor of rank zero, since it has a single component which is unchanged in a coordinate transformation; a vector is considered as a tensor of rank one. Most of the tensors we encounter in this book will be of rank zero (scalars), one (vectors), or two. We will also discuss some fourth-rank tensors due to their importance in continuum mechanics. The inverse relation to (1.44) is

Tij = Qip Qjq Tpq

or

T Tij = Qip Tpq Qqj

(1.48)

Or, in the matrix form, it is written as [T] = [Q][T ][Q]T

(1.49)

We also note that the inverse of (1.47) is

Tij...m = Qip Qjq · · · Qmt Tpq...t

(1.50)

For a second-rank tensor T, the transpose of T is deﬁned as TT = Tij ej ⊗ ei = Tji ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

(1.51)

Cartesian Tensors

15

Tensor T is symmetric if T = TT . Thus, from (1.41) and (1.51), we ﬁnd Tij = Tji for a symmetric T. With reference to the xi system, we have, from (1.44),

= Qiq Qjp Tij = Qjp Qiq Tji = Tpq Tqp

(1.52)

which proves the symmetry with respect to the primed coordinate system. We may conclude that if a tensor is symmetric with reference to one Cartesian system, then it has symmetric components with reference to all Cartesian coordinate systems. Similarly, if T = −TT , then Tij = −Tji , and T is an antisymmetric second-rank tensor. An antisymmetric tensor has components

0 −T12 −T13

T12 0 −T23

T13 T23 0

(1.53)

Finally, we remark that any second-rank tensor can be decomposed into the sum of a symmetric and an antisymmetric tensor, and that this decomposition is unique. We write T = 21 (T + TT ) + 21 (T − TT )

(1.54)

The tensor (T + TT ) is symmetric and the tensor (T − TT ) is antisymmetric. We also mention that an identity tensor I is a special case, where Tij = δij . Thus, the identity tensor is written as I = e1 ⊗ e1 + e2 ⊗ e2 + e3 ⊗ e3

(1.55)

T·I=T

(1.56)

with

EXAMPLE 1.3 Show that an arbitrary tensor A can be expressed as the sum of a spherical tensor (i.e., a scalar times the identity tensor) and a tensor with zero trace (trace A = Aii ). Prove that this decomposition is unique, and that A , the traceless part of A, is given by A = A − 13 (tr A)I, where A is the deviator of A.

Solution Deﬁne B = A − 13 (tr A)I

and

C = 13 (tr A)I

(a)

then A=B+C

© 2005 by Chapman & Hall/CRC Press

(b)

16

Continuum Mechanics and Plasticity

and C is a spherical tensor. We now take the trace of the ﬁrst equation of (a) and get tr B = tr{A − 13 (tr A)I} = tr A − tr 13 (tr A)I = tr A − 13 (tr A)(3) = 0

(c)

Therefore, B is traceless, and from (b) A is the sum of a spherical tensor and a traceless tensor. To prove the uniqueness, we ﬁrst assume that this decomposition is not unique. Then, there exists a spherical tensor D and a traceless tensor E such that A=D+E

(d)

We take the trace of (d) and (b) to ﬁnd tr A = tr D + tr E = tr D = tr C

(e)

because E and B are traceless. Since both D and C are spherical tensors, we write D = DI

and

C = CI

(f)

where both D and C are scalars. Using (e) and taking the trace of (f), we ﬁnd D = C, that is, D = C. This leads to E = B, which proves that the decomposition is unique.

1.5.2

Multiplication of Tensors

Consider a vector s = si ei and a second-rank tensor T = Tij ei ⊗ ej in a coordinate system with base vectors ei . In a new system with base vectors e i = Qji ej , vector s and tensor T have components s i and Tij , respectively, so that s i = Qmi sm ,

Tij = Qri Qsj Trs

(1.57)

The outer product of the vector s and the tensor T is deﬁned by W = s ⊗ T = si ei ⊗ Tjk ej ⊗ ek = si Tjk ei ⊗ ej ⊗ ek = Wijk ei ⊗ ej ⊗ ek

(1.58)

Therefore, the outer product is a third-rank tensor with components given by Wijk = si Tjk . Referring to the new coordinate system, we write

W = s ⊗ T = s i Tjk e i ⊗ e j ⊗ e k = Wijk ei ⊗ e j ⊗ e k

© 2005 by Chapman & Hall/CRC Press

(1.59)

Cartesian Tensors

17

= s T . If we substitute e = Q e into the above equation, we Hence, Wijk ji j i jk i can establish the following transformation formula for the components Wijk :

Wijk = Qpi Qrj Qsk Wprs

(1.60)

We note that the order of multiplication is important and that s ⊗ T = T ⊗ s. Similarly, the outer product of second-rank tensors P and S is R = P ⊗ S = Pij ei ⊗ ej ⊗ Skm ek ⊗ em = Pij Skm ei ⊗ ej ⊗ ek ⊗ em = Rijkm ei ⊗ ej ⊗ ek ⊗ em

(1.61)

and the components are Rijkm = Pij Skm . R is a fourth-rank tensor. In a similar manner, we may form the outer products of three or more tensors or vectors. The outer product of a tensor of rank p with a tensor of rank q is a tensor of rank p + q. We note that the dyadic product of two vectors is a special case, because vectors are tensors of rank one. If we equate the last two indices of third-rank tensor Wijk , we obtain

Wijj = Wi11 + Wi22 + Wi33

(1.62)

in which i is a free index and can take values of i = 1, 2, 3. Using the components transformation formula, we have

Wijj = Qpi Qrj Qsj Wprs = Qpi δrs Wprs = Qpi Wprr

(1.63)

Thus, the components Wprr transform as the components of a vector. This operation of reducing the rank of tensor by two by summing on two indices is called contraction of the tensor. In (1.63), a third-rank tensor is reduced to a vector by contraction. In the case of a tensor of rank n with components Wijkm...rs , if we sum on any pair of its indices such as k = r, then the resulting quantities Wijrm...rs , are the components of a tensor of rank n − 2. In particular, contraction of a second-rank tensor Tij leads to Tii , a scalar. The outer product followed by a contraction leads to an inner product. The inner product of vector s and tensor T is s · T = si Tik em ⊗ em ⊗ ek = si Tik ek

(1.64)

where the relation em ⊗ em = I is applied, in which I is the identity tensor. The inner product formed by a different order is T · s = Tij sj ei ⊗ em ⊗ em = Tij sj ei = si Tki ek

(1.65)

Comparing the two equations given above, we see that s · T = T · s only if T is a symmetric tensor. A similar procedure may be applied to form inner

© 2005 by Chapman & Hall/CRC Press

18

Continuum Mechanics and Plasticity

products of second- and higher-rank tensors. From second-rank tensors U and V, various inner products can be formed, such as U · V = Uij Vjk ei ⊗ ek ,

UT · V = Uji Vjk ei ⊗ ek

(1.66)

These inner products are second-rank tensors. A useful relation involving the inner product is (U · V)T = VT · UT

(1.67)

Using the concept of inner product, we may derive an expression for the components Tij of a second-rank tensor T. Based on (1.41), we may form the following inner product ei · T · ej = ei · Tpq ep ⊗ eq · ej = Tpq ei · ep ⊗ eq · ej = Tpq ei · ep (eq · ej ) = Tpq ei · ep δqj = Tpq δip δqj = Tij

(1.68)

Therefore, the component Tij of tensor T is given by Tij = ei · T · ej

(1.69)

It can be further shown that, from (1.69), we can obtain the following expression T · ej = Tpj ep

1.5.3

(1.70)

The Component Form and Matrices

Matrix operation can be conveniently used to perform transformation of tensor components from one coordinate system to another. For this purpose, we express a tensor equation in terms of a matrix equation in this section. Consider w =T·v

(1.71)

where T transforms vector v into vector w. This equation may be written as wi ei = T · vj ej = vj Tij ei

(1.72)

Thus, the components of (1.72) may be arranged in a matrix equation as [wi ] = [Tij ][vj ]

© 2005 by Chapman & Hall/CRC Press

(1.73)

Cartesian Tensors

19

where wi and vi may be arranged as the elements of two 3 × 1 column matrices [wi ] = [w1 , w2 , w3 ]T , [vi ] = [v1 , v2 , v3 ]T , whereas [Tij ] is a 3 × 3 square matrix. In the case of equation R =S·T

(1.74)

where R, S, and T are second-rank tensors, we write R · ei = S · T · ei

(1.75)

By use of (1.70), we have Rji ej = S · (Tji ej ) = Tji (S · ej ) = Tji Skj ek

or

Rki ek = Tji Skj ek

(1.76)

The component form is now Rki = Skj Tji

(1.77)

[Rik ] = [Sij ][Tjk ]

(1.78)

and the matrix form is

1.5.4

Quotient Law

The quotient law may be used to test whether the elements of a set of quantities A(i, j, k) are components of a tensor. If the inner product (summation over i) between A(i, j, k) and an arbitrary tensor, say bi , is known to yield a tensor Cjk , that is, A(i, j, k)bi = Cjk

(1.79)

then A(i, j, k) is a tensor of type Aijk . Referring to the xi coordinate system, the above equation is written as

A (i, j, k)b i = Cjk

(1.80)

are both tensors, they obey tensor transformation rules given Since b i and Cjk by (1.30) and (1.44), respectively. By substitution, we obtain

A (i, j, k)b i = Qpj Qqk Cpq = Qpj Qqk A(r, p, q)br = Qpj Qqk A(r, p, q)Qri b i

(1.81)

or [A (i, j, k) − Qri Qpj Qqk A(r, p, q)]b i = 0

© 2005 by Chapman & Hall/CRC Press

(1.82)

20

Continuum Mechanics and Plasticity

Since b i is an arbitrary tensor and is generally not zero, we conclude that the quantity within the brackets must vanish. Therefore, A (i, j, k) = Qri Qpj Qqk A(r, p, q)

(1.83)

which is the transformation rule for a tensor of type Aijk . This method may be used to test higher rank tensors.

1.6 1.6.1

Rotation of a Tensor Orthogonal Tensor

The inverse to tensor T is denoted by T−1 , so that T · T−1 = I

and

T−1 · T = I

(1.84)

In the case that the transpose of T is equal to the inverse of T, that is, TT = T−1

(1.85)

then T is said to be an orthogonal tensor. Therefore, for an orthogonal tensor, we have T · TT = I and

TT · T = I

with

det T = ±1

(1.86)

where the “+” sign denotes a proper orthogonal transformation (righthanded coordinate system) and the “−” sign denotes an improper orthogonal transformation (left-handed coordinate system). We now consider the transformation tensor Q discussed in Section 1.3. Since Q satisﬁes (1.86), it is an orthogonal tensor. For the purpose of investigating physical properties of Q, consider two vectors u and v transformed by Q: u¯ = Q · u,

v¯ = Q · v

(1.87)

The inner products Q · u and Q · v may be viewed as linear transformations of vectors u and v by tensor Q. The scalar product of u and v is u¯ · v¯ = (Q · u) · (Q · v) = v · QT · (Q · u) = u · v

(1.88)

which is unchanged under an orthogonal transformation Q. The second equality in (1.88) was a result obtained from the deﬁnition of the transpose of a tensor given by a · (AT · b) = b · (A · a).

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

21

A special case of the above discussion is u = v and u¯ = v. ¯ Here, (1.88) reduces to v¯ · v¯ = (Q · v) · (Q · v) = v · v

(1.89)

|v| ¯ = |v|

(1.90)

or

Therefore, the magnitude of a vector is unchanged by an orthogonal transformation. Furthermore, the angle φ between the two vectors is expressed by cos φ =

u·v u¯ · v¯ = |u||v| |u|| ¯ v| ¯

(1.91)

which means that the angle between the vectors is also unchanged. Thus, an orthogonal transformation rotates a vector and the components Qij are the direction cosines. EXAMPLE 1.4

Show that (Q · u) · (Q · v) = u · v.

LHS = (Qij ei ⊗ ej · uk ek ) · (Qmn em ⊗ en · vp ep ) = Qij Qmn uk vp ei δjk em δnp = Qij uj Qmn vn δim = Qij Qin uj vn = δjn uj vn = uj vj = u · v = RHS Deﬁne the transpose of tensor A by a · (AT · b) = b · (A · a) and shows that it leads to

EXAMPLE 1.5

(AT )T = A. By use of (1.65), we have LHS = a · (ATij bj ei ) = ak ek · ATij bj ei = ak ATij bj δki = ai ATij bj RHS = b · (Aij aj ei ) = bk ek · Aij aj ei = bk Aij aj δki = bi Aij aj = aj Aij bi = ai Aji bj Since the two sides are equal, we obtain ATij = Aji , that is, the transpose of a matrix is the same as the interchange of the two indices. We then have (ATij )T = Aij and we can write AT = ATij ei ⊗ ej = Aji ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

and

(AT )T = Aij ei ⊗ ej = A

22 1.6.2

Continuum Mechanics and Plasticity Component Form of Rotation of a Tensor

In this section, we derive the component form that describes the rotation of a tensor, and we point out that this transformation equation is different from the one which describes the change of bases. In the case of transformation of bases, it has been shown in Sections 1.2.3 and 1.2.5 that the components transform by [vi ] = [Qij ]T [vj ]

[vi ] = [Qij ][vj ]

and

(1.92)

for a vector vi , and by [Tij ] = [Qip ]T [Tpq ][Qqj ]

and

[Tij ] = [Qip ][Tpq ][Qqj ]T

(1.93)

for a tensor Tij . By applying rotation Q to vector v, we write v¯ = Q · v

(1.94)

Thus, vector v is rotated by Q into v. ¯ If the same Q has rotated the bases ei into e i , we can write v¯ = v¯ i e i = Q · v = Q · vi ei = vi (Q · ei ) = vi e i

(1.95)

v¯ i = vi

(1.96)

Therefore,

Equation (1.96) shows that the components of v¯ in e i are the same as those of v in ei . This result is obvious, because both the vector and the coordinate system have been rotated by the same amount and their relative positions remain the same. Consider next the components of v¯ in ei : v¯ = v¯ i ei = Q · v = Q · vi ei = vi Qji ej = vj Qij ei

(1.97)

[v¯ i ] = [Qij ][vj ]

(1.98)

Thus,

Note that this equation is different from (1.92). Equation (1.92) describes the components of v in the e i system, while (1.98) describes the components of the rotated vector v¯ in the ei system. The inverse relation of (1.98) is [vi ] = [Qij ]T [v¯ j ]

© 2005 by Chapman & Hall/CRC Press

(1.99)

Cartesian Tensors

23

We now apply Q to tensor T and write T¯ = Q · T · QT

(1.100)

that is, T¯ is the tensor after rotation. Then, T¯ · e i = T¯ ji e j = Q · T · QT · e i = Q · T · ei = Q · Tji ej = Tji e j

(1.101)

Thus, T¯ ji = Tji

(1.102)

that is, the components of T¯ in e i are the same as those of T in ei , when e i and ei are related by Q. To ﬁnd the component of T¯ with respect to ei , we write T¯ · e i = Q · T · QT · e i = Q · T · ei = Q · Tji ej = Tji Qkj ek

(1.103)

On the other hand, we have T¯ · e i T¯ · Q · ei = T¯ · Qji · ej = Qji T¯ · ej = Qji T¯ kj ek

(1.104)

Equating (1.103) to (1.104), we ﬁnd Qji T¯ kj = Tji Qkj

(1.105)

Multiplying both sides of the equation by Qmi , the resulting equation reduces to T¯ ij = Qim Qjn Tmn

(1.106)

which, in the matrix form, may be written as ¯ = [Q][T][Q]T [T]

(1.107)

Note that this equation (1.107) is different from (1.93) in that the latter describes the components of T in the e i system, while the former describes the components of the rotated tensor T¯ in the ei system.

1.6.3 1.6.3.1

Some Remarks Remark 1 — deﬁnition of Qij

In this book, we deﬁne the components of the transformation matrix by Qij = cos(xi , xj ), in which the ﬁrst subscript refers to the unprimed axis and

© 2005 by Chapman & Hall/CRC Press

24

Continuum Mechanics and Plasticity

the second subscript to the primed axis. The transformation rule for a second-rank tensor T is Tij = Qki Qmj Tkm

(1.108)

In some books, the following equations are used, Tij = Qik Qjm Tkm

(1.109)

where the transformation matrix is deﬁned by Qij = cos(xi , xj ). In this case, the ﬁrst subscript refers to the primed axis and the second subscript to the unprimed axis. Make a note of this difference. 1.6.3.2 Remark 2 — transformation of bases versus rotation of a tensor Note the difference in the transformation equations between a tensor T subjected to the transformation of bases and the tensor T itself undergoing rotation. In the transformation of bases Tij = Qki Qlj Tkl

or

[T ] = [Q]T [T][Q]

(1.110)

and in the rotation of a tensor ¯ = [Q][T][Q]T [T]

(1.111)

For rotation of tensor T in the reversed direction, we substitute [Q] by [Q]T ¯ = [Q]T [T][Q] which is the same as the result and (1.111) reduces to [T] obtained from the rotation of bases. Therefore, rotation of the tensor itself in the opposite direction has the same effect as the rotation of bases. This point is illustrated by Example 1.6. Consider the rotation of a vector v through an angle α into v. ¯ Observing that the magnitude of the vector remains the same in the rotation, that is, |v| ¯ = |v| and, from Figure 1.2, referring to ei , we can write

EXAMPLE 1.6

v¯ 1 = |v| cos(α + β) = |v|(cos α cos β − sin α sin β)

v1 v2 = |v| cos α − sin α = v1 cos α − v2 sin α |v| |v|

(a)

v¯ 2 = |v| sin(α + β) = |v|(sin α cos β + cos α sin β)

v1 v2 = |v| sin α + cos α = v1 sin α + v2 cos α |v| |v|

(b)

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

25 x2 _ v

_ v2 v2

v _ v1

O

v1

x1

FIGURE 1.2 Components of a vector.

We may then use equations (a) and (b) in a matrix equation as v¯ 1 cos α = sin α v¯ 2

− sin α cos α

v1 v2

(c)

The component form of this rotation is from (1.98) v¯ i = Qij vj

(1.98)

Comparing (c) and (1.98), we ﬁnd

cos α sin α

Qij =

− sin α cos α

(d)

However, a rotation of coordinate axes through an angle α in the opposite direction leads to

cos α sin α Qij∗ = (e) − sin α cos α Therefore, from equations (d) and (e), we obtain [Q∗ ]T = [Q]

(f)

The transformation formula in this case is, from (1.92), vi = Qji∗ vj = Qij∗T vj

(g)

Hence, v1 v2

© 2005 by Chapman & Hall/CRC Press

=

cos α sin α

− sin α cos α

v1 v2

(h)

26

Continuum Mechanics and Plasticity

Comparing (c) and (h), we conclude that rotation of a vector through an angle α has the same effect as rotation of axes through the same angle α in the opposite direction. Note that in using (1.98) to obtain v¯ i , the rotation matrix [Q] is obtained by rotating the coordinate axes through angle α in the same direction as the rotation of vector v.

1.6.3.3 Remark 3 — rotation of a vector about an arbitrary direction We now consider the rotation of a vector v about an arbitrary direction with unit vector n and denoted by OA (Figure 1.3(a)). The angle of rotation is α in the sense of the rotation of a right-handed screw advancing in the direction ¯ of n. In the rotation, vector v is rotated into v¯ and particle P is rotated into P. ¯ Hence, P and P lie in a plane normal to line OA, and the plane intersects OA at B. The vector of OB is bn and the length BP = BP = s. From the ﬁgure, we obtain b = n · v = n · v¯

(1.112)

We denote vectors BP and BP by s and s¯ , respectively. Thus, v = bn + s

and

v¯ = bn + s¯

(1.113)

¯ the unit vectors u = s/s and u¯ = s¯ /s are related by In the plane of BPP, u¯ = u cos α + n × u sin α

(1.114)

which can be easily justiﬁed from Figure 1.3(b). Equation (1.114), when multiplied by s, is s¯ = s cos α + n × s sin α (1.115) (a)

(b)

A x3 _ s

B

bn

_

O

_

cos u

P v

v

x2

x1

FIGURE 1.3 Rotation of (a) a vector about a direction; (b) a unit vector.

© 2005 by Chapman & Hall/CRC Press

u

sin

s

_ P

Cartesian Tensors

27

Substituting (1.115) into (1.113), we obtain v¯ = bn + s cos α + n × s sin α = bn + (v − bn) cos α + n × (v − bn) sin α = v cos α + n × v sin α + b(1 − cos α)n = v cos α + n × v sin α + (n · v)(1 − cos α)n

(1.116)

This equation may be written as follows in the component form: v¯ i = vi cos α + eikj nk vj sin α + (1 − cos α)vj nj ni

(1.117)

By comparing with (1.98), we ﬁnd that Qij = δij cos α + eikj nk sin α + (1 − cos α)ni nj

(1.118)

which is the rotation matrix describing the rotation of α about the line OA. In a special case, a rotation about the x3 -axis is obtained by setting n3 = 1 and n1 = n2 = 0 in (1.118) and we obtain

cos α Qij = sin α 0

− sin α cos α 0

0 0 1

(1.119)

A rotation in a reverse sense is denoted by a rotation of −α. In this case, (1.118) gives Qij∗ = δij cos(−α) + eikj nk sin(−α) + (1 − cos(−α))ni nj = δij cos α − eikj nk sin α + (1 − cos α)ni nj = Qji = QijT

(1.120)

Thus, we have shown that a rotation in the reverse sense (−α) can be represented by the transpose of the orthogonal tensor Q, which describes the original rotation (+α). Finally, we note that if the angle α is small, cos α ≈ 1 and sin α ≈ α. Then, equation (1.118) reduces to Qij = δij + αnk ekji

(1.121)

1.6.3.4 Remark 4 — symbolic versus component form Relations between tensor quantities may be expressed either in symbolic or in component form. The former are relations between scalars α, β, . . ., vectors u, v, . . ., and tensors R, S, . . ., and the latter are relations between scalars α, β, . . ., vector components ui , vi , . . ., and tensor components Rij , Sij , . . .. The symbolic notation has the advantage that it emphasizes that the relations are physical

© 2005 by Chapman & Hall/CRC Press

28

Continuum Mechanics and Plasticity

statements and that they are independent of the choice of the coordinate system. On the other hand, the component form is often convenient for carrying out algebraic manipulations. In solving problems, it is always necessary at some stage to introduce a coordinate system and components.

1.7

The Isotropic Tensors

A tensor is isotropic if it has the same components with respect to a Cartesian coordinate system of any orientation. Isotropic tensors of various ranks are given below: Scalar: Every scalar is an isotropic tensor, because the scalar does not have a direction. Vector: There is no nontrivial isotropic vector. Second-rank tensor: The general expression for an isotropic second-rank tensor is Tij = λδij

(1.122)

where λ is a constant. Third-rank tensor: The isotropic third-rank tensor is Tijk = λeijk

(1.123)

Fourth-rank tensor: The most general expression for an isotropic fourthrank tensor is Tijkm = αδij δkm + βδik δjm + γ δim δjk

(1.124)

where α, β, and γ are constants. If Tijkm has the symmetry properties that Tijkm = Tjikm and Tijkm = Tijmk , then from (1.124) Tijkm = Tjikm = αδij δkm + βδjk δim + γ δjm δik = αδij δkm + βδik δjm + γ δim δjk

(1.125)

By subtracting the two expressions in (1.125), and multiplying the resulting equation by δim δjk , we obtain δim δjk γ (δjm δik − δim δjk ) = β(δik δjm − δjk δim )δim δjk

© 2005 by Chapman & Hall/CRC Press

(1.126)

Cartesian Tensors

29

which may be further simpliﬁed to yield γ (δii − δii δjj ) = β(δii − δjj δii )

(1.127)

γ =β

(1.128)

or

Hence, (1.124) may be further reduced to Tijkm = αδij δkm + β(δik δjm + δim δjk )

(1.129)

and we see that the independent constants are now reduced to α and β. EXAMPLE 1.7

Show that there are no nontrivial isotropic vectors.

Proof Introduce a 180◦ rotation of the coordinate system about the x1 -axis as shown in Figure 1.4(a). The transformation matrix for this rotation of axes is

1 [Q] = 0 0

0 −1 0

0 0 −1

(a)

The transformation equation for a vector a is a i = Qji aj . By applying (a), this equation becomes a1 1 a 0 = 2

0 a3 x3

(a)

T 0 a1 a1 0 a2 = −a2 −1 a3 −a3

0 −1 0

x3

(b)

(b)

(c)

x3, x3⬘

x1⬘ x2⬘

O

x2

x1, x1⬘

O

x1 x3⬘

x2, x2⬘

x3⬘

O x1 d x1⬘

d x2

x⬘2

FIGURE 1.4 An 180◦ rotation of coordinate system about (a) the x1 -axis, (b) the x2 -axis, and (c) rotation of a small angle dθ about the x3 -axis.

© 2005 by Chapman & Hall/CRC Press

30

Continuum Mechanics and Plasticity

But, if a vector is isotropic, then a i = ai by deﬁnition. To satisfy this requirement and equation (b), we must have a2 = a3 = 0. However, coordinate axes may be labeled in an arbitrary order. Therefore, a1 = 0 as well. We conclude that there are no nontrivial isotropic vectors.

EXAMPLE 1.8

Tij = λδij .

Show that the isotropic second-rank tensor is given by

Proof Consider a 180◦ rotation of the coordinate system about the x1 -axis (see Figure 1.4(a)). The transformation equation for a second-rank tensor

= Q Q T . By applying (a) of Example 1.7, this equation becomes T is Tpq ip jq ij

T11 [T ] = −T21 −T31

−T12 T22 T32

−T13 T11 T23 = [T] = T21 T33 T31

T12 T22 T32

T13 T23 T33

(a)

The last equality of the above equation is written based on the deﬁnition of an isotropic tensor so that Tij = Tij . Therefore, we conclude that T12 = T21 = 0 and T13 = T31 = 0. We next introduce a 180◦ rotation of the coordinate system about the x2 -axis as shown in Figure 1.4(b). The transformation matrix is

−1 [Q] = 0 0

0 1 0

0 0 −1

(b)

Substituting (b) into the transformation equation for Tij and considering the deﬁnition of an isotropic tensor, we write

T11 [T ] = −T21 T31

−T12 T22 −T32

T13 −T23 T33

isotropic

≡

[T]

(c)

From (c), we conclude that T12 = T21 = 0 and T23 = T32 = 0. Thus, only T11 , T22 , T33 are nonzero. But, since coordinate axis may be labeled in any arbitrary order, we have T11 = T22 = T33 = λ. Therefore, the second-rank isotropic tensor is written as Tij = λδij

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors EXAMPLE 1.9

31

Show that the most general fourth-order isotropic tensor has

the form Tijkm = αδij δkm + βδik δjm + γ δim δjk where α, β, γ are constants. Proof A fourth-order tensor transforms as

Tijkm = Qri Qsj Qtk Qnm Trstn

(a)

There are 34 = 81 components altogether. First, consider any component which contains the index 1 only once. For the coordinate transformation associated with a 180◦ rotation about the x1 -axis and illustrated by Figure 1.4(a), the transformation matrix is given by (a) of Example 1.7. Let i = 1 and use the Qij of Figure 1.4(a), equation (a) becomes

= Qr1 Qsj Qtk Qnm Trstn = Q11 Qsj Qtk Qnm T1stn T1jkm

(b)

But j = 1, so the only nonzero terms of Qsj are Q22 = Q33 = −1, in which j = s; k = 1, so the only nonzero terms of Qtk are Q22 = Q33 = −1, in which k = t; and m = 1, so the only nonzero terms of Qnm are Q22 = Q33 = −1, in which m = n. Thus, (b) becomes

T1jkm = Q11 (−1)(−1)(−1)T1stn = −T1stn = −T1jkm

(c)

= T1jkm , which contradicts the expresIf the tensor is isotropic, then T1jkm sion in (c). Therefore, all the components which contain the index 1 only once are zero, in order to satisfy this requirement. Similarly, all the components that contain the index 2 only once are zero and all the components that contain the index 3 only once are zero. Thus, from the above special transformation, we see that the components of Tijkm are reduced to the following four groups: T1122 , T2211 , T1133 , . . . ; T1212 , T2323 , . . . ; T1221 , T2112 , T2332 , . . . ; and T1111 , T2222 , T3333 . Furthermore, we remark that the coordinate axes may be labeled in an arbitrary order. Thus, a permutation of the indices 1, 2, 3 cannot affect the values of the components of an isotropic tensor. Therefore,

T1122 = T2211 = T1133 = T3311 = T2233 = T3322 = α, say T1212 = T2121 = T1313 = T3131 = T2323 = T3232 = β, say T1221 = T2112 = T1331 = T3113 = T2332 = T3223 = γ , say T1111 = T2222 = T3333 = δ, say

© 2005 by Chapman & Hall/CRC Press

(d)

32

Continuum Mechanics and Plasticity

Consider now a rotation shown in Figure 1.4(c) about the x3 -axis with a very small angle of rotation dθ. The transformation matrix for this case is

cos dθ Qij = sin dθ 0

− sin dθ cos dθ 0

0 1 0 ≈ dθ 1 0

−dθ 1 0

0 0 1

(e)

Equation (e) can be rewritten as

1 Qij = 0 0

0 1 0

0 0 0 + dθ 1 0

−dθ 0 0

0 0 0

or Qij = δij + dθ e3ji

(f)

Only e321 and e312 are not zero in the expressions of e3ji . Note that (f) can also be obtained from (1.121) by letting ni = (0, 0, 1) and α = dθ . Substituting (f) into (a), we have

= (δri + dθ e3ir )(δsj + dθ e3js )(δtk + dθe3kt )(δnm + dθ e3mn )Trstn Tijkm

= (δri δsj + δri dθ e3js + dθ e3ir δsj )(δtk δnm + δtk dθ e3nm + dθ e3kt δnm )Trstn = (δri δsj δtk δnm + δri δsj δtk dθε3mn + δri δsj dθ e3kt δnm + δri dθ e3js δtk δnm + dθ e3ir δsj δtk δnm )Trstn = Tijkm + dθ e3mn Tijkn + dθ e3kt Tijtm + dθe3js Tiskm + dθ e3ir Trjkm = Tijkm + dθ {e3mn Tijkn + e3kt Tijtm + e3js Tiskm + e3ir Trjkm }

(g)

In the above derivation higher order terms in dθ have been neglected since

= Tijkm . Using this dθ is inﬁnitesimal. If the tensor Tijkm is isotropic, then Tijkm information in the last expression of (g), the quantity within the brackets has to be zero. Therefore, e3mn Tijkn + e3kt Tijtm + e3js Tiskm + e3ir Trjkm = 0

(h)

We now investigate the implication of (h). By choosing i = 1, j = k = m = 2, (h) becomes e321 T1221 + e321 T1212 + e321 T1122 + e312 T2222 = 0 or T2222 = T1221 + T1212 + T1122

© 2005 by Chapman & Hall/CRC Press

(i)

Cartesian Tensors

33

Substituting (d) into (i), we get δ =α+β +γ

(j)

Other choices of indices i, j, k, m in (h) gives either the same relation (j) or relations that are identically satisﬁed, if we use the isotropy conditions previously obtained. Thus, we have shown that there are only three distinct components of an isotropic fourth-rank tensor, namely α, β and γ ; and Tijkm can be written as Tijkm = αδij δkm + βδik δjm + γ δim δjk

(k)

All components of isotropic Tijkm can be found from (k). Examples are T1122 = αδ11 δ22 + βδ12 δ12 + γ δ12 δ12 = α T2233 = αδ22 δ33 + βδ23 δ23 + γ δ23 δ23 = α T1221 = αδ12 δ21 + βδ12 δ21 + γ δ11 δ22 = γ and so on. EXAMPLE 1.10 Using the expression of an isotropic fourth-rank tensor, reduce the generalized Hooke’s law to an isotropic relation. Linearly elastic materials are governed by the generalized Hooke’s law as

σij = Cijkm εkm

(a)

where σij and εij are second-rank tensors and Cijkm is a fourth-rank tensor. Due to the symmetric property of σij and εij , we ﬁnd Cijkm = Cjikm and Cijkm = Cijmk . If the material is isotropic, tensor Cijkm should be an isotropic tensor. Thus, from (1.130), Cijkm = λδij δkm + µ(δik δjm + δim δjk )

(b)

Substituting (b) into (a), we obtain σij = λδij δkm εkm + µδik δjm εkm + µδim δjk εkm = λεkk δij + µεij + µεji = λδij εkk + 2µεij

(c)

In the derivation, the symmetric property of εij = εji was used. λ and µ are known as Lamé constants.

© 2005 by Chapman & Hall/CRC Press

34

1.8 1.8.1

Continuum Mechanics and Plasticity

Vector and Tensor Calculus Tensor Field

If to every point xi of region R there corresponds a scalar φ, then we have a scalar ﬁeld φ(xi ) deﬁned over R. An example of the scalar ﬁeld is the temperature ﬁeld, where the temperature in the region R of a continuum is known and may vary from point to point. Similarly, we can deﬁne a vector ﬁeld. If to every point xi of region R corresponds a vector vi , then we have a vector ﬁeld vi (xj ) deﬁned over R. Force ﬁeld, displacement ﬁeld, and velocity ﬁeld are examples of vector ﬁeld. A tensor ﬁeld can be similarly deﬁned. Stress ﬁeld and strain ﬁeld are tensor ﬁelds of rank two.

1.8.2

Gradient, Divergence, Curl

We consider differentiation and integration in the study of vector calculus. Differentiation is discussed in this section and integration in a later section. There are three kinds of differentiation: the gradient, the divergence, and the curl. The gradient of a scalar ﬁeld φ, denoted by Grad φ, is a vector whose components are Grad φ =

∂φ ∂φ ∂φ , , ∂x1 ∂x2 ∂x3

T

= a vector

(1.130)

In other notations, Grad φ may be denoted by −−−−→ ∂φ Grad φ = ek = φ,i ek = ∇φ ∂xk

(1.131)

“del” is used in the last expression of (1.131). In our The differential operator ∇ notation ∇ is = ek ∂ ∇ ∂xk

(1.132)

is not commutative with respect to the quantity which it The operator ∇ operated in the sense that = φ ∇ ∇φ

(1.133)

1.8.2.1 Geometric signiﬁcance of the gradient The value of the scalar ﬁeld φ(xk ) deﬁned over the region R varies in general with xi . The expression, φ(xk ) = constant, deﬁnes a set of surfaces on which φ

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

35

P(xi ) ∆xi

x3

Surface S on which is Constant

x2

O

P⬘(xi + ∆xi)

x1 FIGURE 1.5 A constant φ surface.

is constant. Consider a point P(xi ) and a neighboring point P (xi + xi ) on the surface S, and denote the vector from P to P by xi as shown in Figure 1.5. Since both points are on the same surface, φ evaluated at the two points are the same, and we write φ(P ) − φ(P) = 0

or φ(xi + xi ) − φ(xi ) = 0

(1.134)

Expanding the function φ(xi + xi ) in Taylor’s series, we have φ(xi + xi ) = φ(xi ) + φ,i xi + 0(xi )2

(1.135)

But, xi has a small value and we may take it as small as possible in the sense of calculus. In this way, we may neglect the higher order terms in xi and keep only the ﬁrst-order term in (1.135). Therefore, (1.134) becomes φ(P ) − φ(P) = φ,i xi = 0

(1.136)

and this is true for any vector xi through P lying on the surface S. Hence, the gradient φ,i is normal to the surface S. 1.8.2.2 Differential operators on vectors There are two differential operators on vector vi which are well known. They are the divergence and the curl. The divergence of vector v is written as Div v ≡ vi,i =

∂vi = ∂xi

∂v1 ∂v2 ∂v3 + + ∂x1 ∂x2 ∂x3

(1.137)

the divergence is In terms of ∇, · v = ek Div v = ∇

© 2005 by Chapman & Hall/CRC Press

∂ ∂vm · (vm em ) = ek · em = δkm vm,k = vk,k ∂xk ∂xk

(1.138)

36

Continuum Mechanics and Plasticity

The curl of vector v, denoted by vector w, is × v = ek ∂ × (vm em ) = ek × ej vj,k = ekjm em vj,k w = Curl v = ∇ ∂xk

(1.139)

and its components are Wm = (Curl v)m = ekjm vj,k = emkj vj,k

(1.140)

in which vj,k is the velocity gradient if vi is the velocity. The velocity gradient is an important kinematic quantity and is discussed in Chapter 3. From (1.140), we have w1 = v3,2 − v2,3 . Vector wm is the dual vector of tensor vj,k except for a constant multiple factor. Dual vectors are discussed in Chapter 3. are given below: Some operations using the operator ∇ (a) (b)

∂ · (∇φ) ∇ = ej · (ek φ,k ) = ej · ek φ,kj = δjk φ,kj = φ,kk = ∇ 2 φ ∂xj × (∇φ) = Curl Grad φ = ej ∂ × (ek φ,k ) = ej × ek φ,kj ∇ ∂xj

(1.141)

= ejkm em φ,kj = ejk1 e1 φ,kj + ejk2 e2 φ,kj + ejk3 e3 φ,kj = e231 e1 φ,32 + e321 e1 φ,23 + · · · = 0

(1.142)

We note that ejk1 is antisymmetric and φ,kj is symmetric such that their inner product is zero. For the same reason the other two terms involving m = 2 and m = 3 are also zero. The above result can also be seen easily by expanding out each term as in the last equality. Since e231 = 1 and e321 = −1, the terms of the last equality cancel out in pairs. (c)

∂ ∂ ∇ · (∇ × v) = ej · ek × (er vr ) ∂xj ∂xk = ej

∂ ∂ · [ek × er vr,k ] = ej · [ekrs vr,k es ] ∂xj ∂xj

= ej · ekrs es vr,kj = δjs ekrs vr,kj = ekrj vr,kj = 0

(1.143)

The last equality is again obtained by observing that the inner product of an antisymmetric tensor with a symmetric tensor is zero. (d)

× (∇ × v) = es ∂ × [ekjm vm,j ek ] = es × ek ekjm vm,js ∇ ∂xs = −eksr er ekjm vm,js = −{δsj δrm − δsm δrj }vm,js er = −vm,ss em + vs,js ej = −vm,ss em + (vs,s ),j ej ∇ · v) = −∇ 2 v + ∇(

© 2005 by Chapman & Hall/CRC Press

(1.144)

Cartesian Tensors

37

Note that ∇ 2 v is written as:

2 · ∇)v = ei ∂ · ej ∂ (vk ek ) = ∂ vk (ei · ej )ek (∇ ∂xi ∂xj ∂xi ∂xj =

∂ 2 vk ek = vk,jj ek ∂xj ∂xj

(1.145)

By use of (1.39), we have · ∇)v = v⊗∇ ·∇ (∇

(1.146)

Therefore, ∇ 2 v can be written in either of the following two forms ·∇ = (∇ · ∇)v ∇ 2v = v ⊗ ∇

(1.147)

(e) There are two forms of the divergence of tensor T. They are: ∂Tpq ∂Tpq · T = ∂ ek ·(Tpq ep ⊗ eq ) = ∇ (ek · ep )eq = eq ∂xk ∂xk ∂xp = T·∇

∂Tqp eq ∂xp

(1.148)

(1.149)

The two divergences are in general different, but they are the same if the =∇ ·T, and this relationship tensor T is symmetric. We can further write TT · ∇ is similar to that of the inner product between a vector and a second-rank tensor presented in (1.64) and (1.65).

1.8.3

The Theorem of Gauss

In continuum mechanics, an important application of the theorem of Gauss is to change an area integral into a volume integral and vice versa. Consider a body of surface S and volume V, with surface element dS and volume element dV shown in Figure 1.6, the Gauss theorem is written as S

φni dS =

S

φ,i dV

for scalar φ

(1.150)

vj ni dS =

S

V

V

vj,i dV

ai1 i2 ...iN nj dS =

© 2005 by Chapman & Hall/CRC Press

for vector vj

(1.151)

V

ai1 i2

... iN ,j

dV

for tensor ai1 ...iN

(1.152)

38

Continuum Mechanics and Plasticity

dV nAi

ni

A

dS P ui

P⬘ B

x3

nBi x2

O x1

FIGURE 1.6 Surface and volume elements in a deformable body.

Proof We prove (1.150) here. The proofs of (1.151) and (1.152) can be similarly obtained. Ascalar ﬁeld φ is deﬁned in V and we divide the body into an inﬁnite number of parallel inﬁnitesimal cylinders. A generic inﬁnitesimal cylinder is shown in the Figure 1.6 with ends Aand B. Ends Aand B are parts of the surface B area S of the body and has unit outward normal nA i or ni , respectively. We

now consider two neighboring points P(xi ) and P (xi +dxi ) in the inﬁnitesimal cylinder. The unit vector along the generator of the cylinder is denoted by ui as shown in the Figure 1.6 and is a constant. The differential dφ is given by

dφ =

∂φ ∂φ ∂φ dx1 + dx2 + dx3 = φ,i dxi = ui φ,i ds ∂x1 ∂x2 ∂x3

(1.153)

where ds is the length of dxi . If this expression is integrated over the inﬁnitesimal cylinder, we ﬁnd φB − φA = ui

B A

φ,i ds

(1.154)

The cross-section of the cylinder is dT = (−ni ui dS)A = (ni ui dS)B

© 2005 by Chapman & Hall/CRC Press

(1.155)

Cartesian Tensors

39

Note that ni ui is negative at A and positive at B. Multiplying both sides of (1.154) by (1.155), we obtain φB (ni ui dS)B − φA (−ni ui dS)A = ui

B

φ,i ds dT

(1.156)

φ,i dV

(1.157)

A

which may be rewritten as (φni ui dS)B + (φni ui dS)A = ui

B A

or ui

dSA +dSB

φni dS = ui

Vcylinder

φ,i dV

(1.158)

In deriving (1.158), we observe that because dSA and dSB are small surface areas, we assume that φ and ni are constants in dS, then ui

dSA +dSB

φni dS = ui

dSA

φni dS + ui

∼ = ui (φni )A

dSA

dSB

φni dS

dS + ui (φni )B

dS dSB

= (φni ui dS)A + (φni ui dS)B = LHS of (1.157)

(1.159)

Equation (1.158) is valid for the inﬁnitesimal cylinder considered. For the whole body, we sum over all inﬁnitesimal cylinders and obtain

Sall

φni dS =

Vall

φ,i dV

(1.160)

which proves equation (1.150). We remark that the theorem of Gauss is still valid for multiply connected region. In that case, we have to make branch cuts to prove the theorem. Some special cases of the theorem are listed below: 1. Expressions in 3-D: V

Div v dV =

© 2005 by Chapman & Hall/CRC Press

S

n · v dS

(divergence theorem)

(1.161)

40

Continuum Mechanics and Plasticity S

n

L FIGURE 1.7 Contour and surface.

This equation can be obtained by putting i = j in (1.151).

V

Curl v dV =

S

n × v dS

(1.162)

This equation can be obtained by multiplying both sides of (1.152) by ekij . 2. Expressions in 2-D: S

Div v dS =

L

n · v dL

Curl v dS = n × v dL S L v · dL = n · Curl v dS (Stoke’s theorem) L

(1.163) (1.164) (1.165)

S

In the two-dimensional case, the theorem changes the surface integral into the line integral and vice versa. Figure 1.7 shows the contour L and the surface S. In (1.165), the left integral is the circulation of v along the contour L and n is the unit outward normal on the surface S.

References 1. Malvern, L.E., Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Englewood Cliffs, NJ, 1969. 2. Spencer, A.J.M., Continuum Mechanics, Longman, London and New York, 1980. 3. Lai, W.M., Rubin, D., and Krempl, E., Introduction to Continuum Mechanics, Pergamon Press, New York, 1974. 4. Fung, Y.C., First Course in Continuum Mechanics, Prentice-Hall, Englewood Cliffs, NJ, 1994. 5. Chadwick, P., Continuum Mechanics, George Allen & Unwin, London, 1976.

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

41

Problems (1) The equations of motion are ∂Tsr + ρbr = ρar ∂xs Write out the equations in conventional notations, that is, use x = x1 , y = x2 and z = x3 . (2) Prove that δij δij = 3 eijk Aj Ak = 0 δij eijk = 0 (3) If Tij is symmetric, evaluate the expressions (a) eijk Tjk and (b) eijk eist Tkt . (4) Given that

1 [Sij ] = −1 2

0 3 −1

0 2 1

evaluate (a) Sii , (b) Sjj , (c) Sij Sij , (d) Sjk Skj , (e) Smn Snm (5) Using the e–δ identity, show that eikm ejkm = 2δij

and

eijk eijk = 6

(6) Given vectors u = ui ei and v = vi e, show that the components of w = u×v are w1 = u2 v3 − u3 v2 ,

w2 = u3 v1 − u1 v3 ,

w3 = u1 v2 − u2 v1

(7) If ui = eijk vj wk and vi = eijk sj tk , show that ui = sk wk ti − tk wk si . (8) Find the transformation matrix [Q] if the coordinate system is rotated through a positive 90◦ about the positive x3 -axis. (9) Can the matrices

1 0 0

0 2 0

0 0 3

and

be matrices of the same tensor? Why?

© 2005 by Chapman & Hall/CRC Press

1 0 0

0 1 0

0 0 3

42

Continuum Mechanics and Plasticity

(10) The components of a second-rank tensor with respect to the xi coordinate system are

4 [A] = 3 0

3 −1 0

0 0 1

Find the components of the same tensor with respect to the xi , coordinate system, if x3 = x3 and x1 is making a 30◦ counterclockwise angle with the x1 -axis. (11) Prove that the decomposition of a tensor into a symmetric and an antisymmetric part is unique. (12) Show that the value of Aij xi xj is unchanged if Aij is replaced by its symmetric part. (13) If Aij is a tensor and Bij is a symmetric tensor, show that the product Aij Bij is independent of antisymmetric part of Aij . (14) In the coordinate transformation from xi to xi , the transformation rule for the

= Q Q T , where Q is the transcomponents of a second-rank tensor is Tpq ip jq ij ij formation matrix. Derive the reversed expression of this equation, that is, express Tij in terms of Tij and Qij . (15) Investigate the inﬂuence of the coordinate transformation x1 = −x1 , x2 = x2 , x3 = x3 on the components of a tensor T. (16) Prove that ei ⊗ ei = I where I is the identity tensor. (17) Show that det(ei ⊗ ei ) = 1 and det(e1 ⊗ e1 ) = 0. (18) Show that (a ⊗ b) · (c ⊗ d) = (b · c)(a ⊗ d). (19) Show that if the components of tensor T are Tij = δij in the xi coordinate system, then the components are Tij = δij in the xi coordinate system. (20) A rigid body is rotated through positive 90◦ about x2 -axis by the right-handed screw rule. Find a matrix representing this rotation. (21) Suppose that the body of the previous problem is subsequently given a 90◦ rotation about the x1 -axis by the right-hand screw rule, ﬁnd the matrix representation of the resultant rotation. If the position of a particle P on the rigid body was (0, 1, 1), what is its position after two rotations? (22) Reverse the order of above two rotations and ﬁnd the ﬁnal position of P. (23) A rigid body undergoes two rotations. The ﬁrst is a rotation through a positive 30◦ angle about a direction speciﬁed by the unit vector n = 0.286e1 +0.857e2 + 0.429e3 with respect to a ﬁxed Cartesian coordinate system with origin at O. This rotation is followed by a second rotation which rotates a positive 90◦ angle about a direction speciﬁed by the unit vector m = −0.667e1 −0.667e2 +0.333e3 . Both axes of rotation pass through the origin O. If the position of a point P on the rigid body is (1, 1, 0), what is its position after the two rotations?

© 2005 by Chapman & Hall/CRC Press

Cartesian Tensors

43

(24) The velocity ﬁeld vi (x) of a rigid body can be written as vi = bi + eijk cj xk , where the vectors bi and cj do not depend on the position of the considered particle. Show that the curl of this velocity ﬁeld is 2ci while the divergence of the velocity ﬁeld vanishes. (25) In the vector ﬁeld v(x), let there exist a surface on which v = 0. Show that, at an arbitrary point of this surface, Curl v is tangential to the surface or vanishes, while Div v is given by the rate of change of the normal component of v in the direction of the normal of the surface. (26) A tensor M transforms every vector into its mirror image with respect to the plane whose normal is √ 2 n= (e + e2 ) 2 1

(a) Find the matrix of M. (b) Use this linear transformation to ﬁnd the mirror image of a vector a = e1 + 2e2 . (Note that this is not a case of rotation. This case is known as reﬂection.) (27) Let φ(x, y, z) and ψ(x, y, z) be scalar functions of positions, and let v(x, y, z) and w(x, y, z) be vector functions of position. By writing in the component form, verify the following identities: + ψ) = ∇φ + ∇ψ (a) ∇(φ (b) Div(v + w) = Div v + Div w · v + φ(Div v) (c) Div(φw) = (∇φ) (28) Consider the integral L e3ij ni vj dL, where L is the closed boundary of a plane surface S with normal (0, 0, 1); vi is a vector; ni is the outward normal of the contour L. Show that this integral is the circulation of vector vi along L denoted by L v · dL.

© 2005 by Chapman & Hall/CRC Press

2 Stress

2.1

Introduction

When forces are applied to a body, they cause the body to deform. In this chapter, we study about the forces and the intensity of forces, and in the next chapter, we study the deformation of the body. The intensity of forces is known as stress, and it is the stress, not the force, that plays an important role in the quantiﬁcation of effect due to forces. A force may be applied to a small area, and a distributed load of the same resulting magnitude may be applied to a larger area. The effects of the two cases are different locally because the stresses are not the same. The concept of stress needs to be deﬁned, and it can be represented by a second-rank tensor. We investigate the properties of stress in this chapter and we also list some references [1–6] for additional reading.

2.2

Forces

Consider a body of volume V and surface S as shown in Figure 2.1. A generic material element of the body has a volume dV, and a generic surface element has area dS and an outward normal n. There are four types of “forces” that act on a body. The “forces” include, in a broad sense, the forces and moments. The four types of “forces” are: 1. Body forces: These are forces whose magnitudes are proportional to the mass contained in the material element of the body. The body forces may either be deﬁned per unit mass or per unit volume. An important example of body force is the gravity force, which is expressed as ρg dV, where ρ is the density; and g is the gravitational acceleration. 2. Surface forces: These forces act on the surface element dS of the body. Externally applied loads, contact forces between bodies, and reactions are examples of surface forces, out of which surface tractions or stress vectors may be deﬁned. The stress vector is the stress force per unit area. 45

© 2005 by Chapman & Hall/CRC Press

46

Continuum Mechanics and Plasticity

dV

t(n)

b dS

r

n

x3

x2

O x1 FIGURE 2.1 Body force and surface traction.

3. Body moments: These are moments applied to the volumetric element dV. It is usually expressed in terms of moment per unit volume, or moment per unit mass. 4. Couple stress: The couple stress is the moment per unit area applied on a surface. In this chapter, we consider only the ﬁrst two types of forces — body and surface forces. These are the most common forces that appear in the study of thermo-mechanical behavior of engineering materials. The remaining two types of “forces” are not important in the case of mechanical behavior of materials, but they play an important role in the case of a polarized dielectric solid under the action of an electric ﬁeld. They also could be signiﬁcant in the study of bones or materials with microstructures, and/or from the action of an external magnetic ﬁeld. Even without external couples, couple stress can arise from interactions between adjacent parts of the material other than central-force interaction. In this chapter, we study the basic principles and methods of continuum mechanics.

2.3

Stress Vector

The stress vector is also known as the surface traction. Consider the surface element dS shown in Figure 2.1, where the surface force applied to the element is p. We write p = t(n) dS

© 2005 by Chapman & Hall/CRC Press

(2.1)

Stress

47

where p dS→0 dS

t(n) (xk ) = lim

(2.2)

where t(n) is the stress vector, which is the intensity of surface force and has a unit of force per unit area. The stress vector is a function of position, a function of xi , and in general it is different from one point on the surface of the body to another point. The outward normal of dS is denoted by n, and t(n) and n are not in the same direction.

2.4

The Stress Tensor

We now consider the stress inside the body, let us cut out a tetrahedron of inﬁnitesimal size from a body, as shown in Figure 2.2. The triangular surface dS(n) , with outward normal n, is inclined to the coordinate axes. The remaining three sides of the tetrahedron, dS1 , dS2 , and dS3 , lie on the coordinate surfaces, and their outward normals are −e1 , −e2 , and −e3 , respectively. The stress vectors acting on these surfaces are −t1 , −t2 , and −t3 , respectively. The negative sign indicates that these forces act on the surfaces with negative normals. Let us now consider the force equilibrium of the tetrahedron. For this we need to sum the surface forces acting on all faces of the tetrahedron and the body force ρb dV acting on the mass of the tetrahedron and then set the result to zero. We obtain −t1 dS1 − t2 dS2 − t3 dS3 + ρb dV + dS(n) t(n) = 0 x3 –t1

t(n)

∆S1 O –t2

n

∆S2

x2 ∆S

3

∆S (n)

∆V b –t3 x1 FIGURE 2.2 Stress vectors.

© 2005 by Chapman & Hall/CRC Press

(2.3)

48

Continuum Mechanics and Plasticity

On applying a limiting process, the volume dV tends to zero, but successive smaller elements retain their surfaces parallel. Since the volume and the area are of the third order and the second order of smallness in length, respectively, in the limit, the term ρb dV becomes a higher order of smallness relative to the other terms and can be ignored. Thus, (2.3) becomes t1 dS1 + t2 dS2 + t3 dS3 = dS(n) t(n)

(2.4)

Since dSi are projections of the inclined surface dS(n) onto the coordinate surfaces, we have dSi = ni = cos(xi , n) dS(n)

(2.5)

By use of (2.5), (2.4) reduces to t(n) = ti ni

(2.6)

Referring to (2.6), we emphasize that t(n) is a vector acting on the inclined surface dS(n) , and ti are vectors acting on the surfaces dSi . Each of these vectors can be expressed by its components referred to the coordinate axes xi . To do this, we write (n)

t(n) = tk ek

and

ti = σik ek

(2.7)

(n)

where tk are the components of t(n) ; and σik are the components of ti in the coordinate directions. Substituting (2.7) in (2.6), we obtain (n)

tk ek = σik ek ni

or

(n)

tk = σik ni

(2.8)

which, in the matrix form, is written as [t(n) ] = [σ ]T [n]

(2.9)

The quantities σik are also components of a second-rank tensor from the quotient law discussed in Section 1.5.4. Comparing (2.8) with (1.80), we infer that ni is an arbitrary tensor (It is arbitrary, since we may choose the direction of (n) the inclined surface.) and tk is a tensor. Therefore, we conclude that σik is a tensor. The importance of (2.8) is that it relates the stress vector t(n) acting on a plane with unit normal n to the stress tensor σ in the material element. Knowing n and t(n) , σ may be found from the equation. The stress tensor is expressed using the tensor bases as σ = σij ei ⊗ ej

© 2005 by Chapman & Hall/CRC Press

(2.10)

Stress

49 x2 22 21

23

12

32 11 31

13

x1

33

x3 FIGURE 2.3 Stress tensor components.

and in the symbolic notation, (2.8) is written as t(n) = σT · n

(2.11)

We now discuss the meaning of the stress components σij . These are intensity of forces (force per unit area) along the coordinate directions. They vary with the location in the body and their magnitudes and speciﬁc characteristics depend on the geometrical shape of the body and the loading condition (surface traction). To determine the distribution of stress in the body, we need to solve a boundary-value problem, by specifying the boundary conditions. However, this problem will not be discussed in this chapter. Instead, we concentrate on understanding the nature of stress at a given point, and consider the stress at a point. To visualize the stress at a point, we consider a parallelepiped cut out from the body. The size of the parallelepiped is not important as long as it is inﬁnitesimal. This is so, because, in the sense of calculus, we consider the stress at a point by taking the limit with the size of the parallelepiped of approaching zero. Figure 2.3 shows the components σij applied on the faces of the parallelepiped. The ﬁrst subscript denotes the direction of the normal to the considered plane and the second subscript denotes the direction in which the stress component acts. σ11 , σ22 , σ33 are the normal stresses and σ12 , σ21 , σ23 , σ32 , σ13 , σ31 are the shear stresses. For given n and t(n) on an inclined plane, show by coordinate transformation that σij are components of a tensor. With the orientation of the inclined surface ﬁxed, let us vary the choice of the coordinate system, so that we have xi and xi coordinate systems. In this exercise, n and t(n) remain ﬁxed. Using (2.6) and referring to the two coordinate

EXAMPLE 2.1

© 2005 by Chapman & Hall/CRC Press

50

Continuum Mechanics and Plasticity

systems, we have ti ni = t(n) = ti n i

(a)

Referring ti to the xi axes and ti to the xi axes, we write σij ej ni = σik e k n i

(b)

But, from (1.28) and (1.32), ej = Qjk e k

ni = Qip n p

and

(c)

So, by substitution σij Qjk e k Qip n p = σik e k n i

or

σij Qjk Qip n p = σik n i

(d)

Since this relation is true for all n, the above equation reduces to σij = Qki Qmj σkm

[σ ] = [Q]T [σ ][Q]

or

(e)

Therefore, we can conclude that σij are components of a second-rank tensor because they obey the transformation rule of a second-rank tensor. EXAMPLE 2.2

Show that the components of tensor equation (2.11) is (2.8). (n)

LHS of (2.11) = ti ei

(a)

RHS of (2.11) = σji ei ⊗ ej · nk ek = σji nk ei δlk = σji nj ei

(b)

Equating (a) with (b), we obtain (2.8).

2.5

Equations of Equilibrium

We derive the equations of equilibrium by summing all the forces applied to a body and reducing it to the local form. Refer to the body of Figure 2.1, and note that every portion of this body is in equilibrium. Consider that only surface tractions and body force apply to this body. The “global form” of the equations of equilibrium is then

V

© 2005 by Chapman & Hall/CRC Press

ρbi dV +

(n)

S

ti

dS = 0

(2.12)

Stress

51

By use of (2.8), (2.12) becomes

V

ρbi dV +

S

σji nj dS = 0

(2.13)

We now use the Gauss theorem to change the second integral of (2.13) into a volume integral. Then, we obtain V

(ρbi + σji,j ) dV = 0

(2.14)

Since the region of integration V is arbitrary and every part of the medium is in equilibrium, we conclude that the integrand must be zero to make the integral zero. Thus, ρbi + σji,j = 0

or

∂σji + ρbi = 0 ∂xj

(2.15)

Equations (2.15) are the equations of equilibrium in the local form, and they may be expanded into a familiar form as ∂σ21 ∂σ31 ∂σ11 + + + ρb1 = 0 ∂x1 ∂x2 ∂x3 ∂σ12 ∂σ22 ∂σ32 + + + ρb2 = 0 ∂x1 ∂x2 ∂x3

(2.16)

∂σ13 ∂σ23 ∂σ33 + + + ρb3 = 0 ∂x1 ∂x2 ∂x3 Show that the mean value theorem may be used to reduce the “global form” of the equations of equilibrium to the “local form.” The mean value theorem is

EXAMPLE 2.3

b a

f (x) dx = (b − a)f (ξ ),

with a ≤ ξ ≤ b

(a)

On the right-hand side of (a), the function f (ξ ) is evaluated at some point in the range of a and b. In the case of equation (2.14), the function f is ρbi + σji,j , which is evaluated at some interior point in V. Thus, (2.14) becomes V

(ρbi + σji,j ) dV = V(ρbi + σji,j ) = 0

(b)

Since V = 0, we obtain ρbi + σji,j = 0

© 2005 by Chapman & Hall/CRC Press

(c)

52

2.6

Continuum Mechanics and Plasticity

Symmetry of the Stress Tensor

The stress tensor is symmetric, that is, σ12 = σ21 , σ23 = σ32 , and σ31 = σ13 , so that the nine components of σij reduce to six independent components. This is not an assumption, but is the result of conservation of angular momentum. A simple way to show this is to project the stresses on the parallelepiped of Figure 2.3 onto a coordinate plane, say the (x1 − x2 ) plane, as shown in Figure 2.4. By summing moment about O, we get σ12 = σ21

(2.17a)

Similarly, by projecting the stresses and the parallelepiped onto the other two coordinate planes and summing moments about O, we ﬁnd σ23 = σ32

and

σ31 = σ13

(2.17b)

A rigorous proof of the symmetry of the stress tensor may be obtained by considering the conservation of angular momentum. We consider the general case that the body moment per unit volume Mi is included in the derivation. The effect of Mi will then be discussed. Referring to Figure 2.1, we have ρ(r × b)i = ρeijk xj bk = moment of ρbk about the origin (n)

(n)

(r × t(n) )i = eijk xj tk = moment of tk about the origin

(2.18) (2.19)

Summing moment about the origin O, we write V

ρeijk xj bk dV +

S

(n) eijk xj tk dS +

V

Mi dV = 0

x2 22 21 12 11

11 12 Ο

x1

21 22

FIGURE 2.4 2 D stress components.

© 2005 by Chapman & Hall/CRC Press

(2.20)

Stress

53

The second integral in (2.20) may be transformed into a volume integral by use of the Gauss theorem. Thus, (2.20) becomes ∂ ρeijk xj bk + (2.21) (eijk xj σrk ) + Mi dV = 0 ∂xr V The second term in (2.21) is ∂xj ∂σrk = eijk (σjk + xj σrk,r ) = eijk σjk + eijk xj (−ρbk ) σrk + xj eijk ∂xr ∂xr (2.22) where the last expression was obtained from the equations of equilibrium. Hence, (2.21) becomes [ρeijk xj bk + eijk σjk − ρeijk xj bk + Mi ] dV = 0 (2.23) V

which leads to V

(eijk σjk + Mi ) dV = 0

(2.24)

Since the integrand is continuous and the volume V is arbitrary, we obtain eijk σjk + Mi = 0

(2.25)

We now discuss the meaning of (2.25) in two different cases as follows: 1. If the body moment is absent, that is, Mi = 0, then (2.25) reduces to eijk σjk = 0

(2.26)

For i = 1, (2.26) gives e123 σ23 +e132 σ32 = 0. Since e123 = 1 and e132 = −1, we obtain σ23 = σ32 . For i = 2, (2.26) leads to σ13 = σ31 ; and for i = 3, (2.26) leads to σ21 = σ12 . Therefore, we write σij = σji

(2.27)

2. If Mi = 0, then σij = σji , and the stress tensor is not symmetric.

2.7

Principal Stresses

If we pass a plane through the parallelepiped of Figure 2.3 and cut the element into two parts, then one of the two parts may be viewed as a tetrahedron

© 2005 by Chapman & Hall/CRC Press

54

Continuum Mechanics and Plasticity x3

t ( n) n x2

O

x1

FIGURE 2.5 Stress vector on an inclined plane.

shown in Figure 2.5. Within the tetrahedron the stress is σij as deﬁned in Figure 2.3. The unit normal to the plane is n, and the associated stress vector t(n) may be found from (2.8) or (2.11). Generally, the two vectors n and t(n) have different directions as shown in Figure 2.5. We now inquire whether we can cut the parallelepiped in a speciﬁc direction (ﬁnd an n), such that n and t(n) have the same direction. If such an n exists, then t(n) = λn, where λ is the magnitude of vector t(n) . In this event, using (2.6), we obtain ti ni = λn

(2.28)

Substituting (2.7) into (2.28), we have σij ej ni = λnj ej

and

σij ni = λnj

(2.29)

which may be written as (σij − λδij )ni = 0

(2.30)

The solution of this set of equations would make t(n) lie in the direction of n. The solution includes ﬁnding the direction n and the magnitude λ. Mathematically speaking, (2.30) is a statement of the eigenvalue problem. The trivial solution ni = 0 of the homogeneous equations (2.30) does not satisfy the unit vector condition n21 + n22 + n23 = 1, so it cannot be our answer.

© 2005 by Chapman & Hall/CRC Press

Stress

55

The condition that a nontrivial solution exists for ni is that σ11 − λ |σij − λδij | = σ21 σ31

σ13 σ23 = 0 σ33 − λ

σ12 σ22 − λ σ32

(2.31)

Expanding the determinant in (2.31), we obtain λ3 − J1 λ2 + J2 λ − J3 = 0

(2.32)

where J1 = tr(σij ) = σii

σ J2 = tr cofactor(σij ) = 22 σ32

σ23 σ11 + σ33 σ31

σ13 σ11 + σ33 σ21

σ12 σ22

(2.33)

J3 = det σij The quantities J1 , J2 , and J3 are called the principal invariants of σij , because they remain invariant with a rotation of the coordinate system. Referring to two coordinate systems xi and xi , the invariants transform as σii = σii ,

tr cofactor(σij ) = tr cofactor(σij ),

det σij = det σij

(2.34)

Therefore, J1 = J1 , J2 = J2 and J3 = J3 . The stress invariants are further discussed in Section 2.11. Note that stresses (λ1 , λ2 , λ3 ) found by solving the characteristic equation (2.32) are called principal stresses and are often denoted by (σ1 , σ2 , σ3 ). In the mathematical language, λr (r = 1, 2, 3) are (r) eigenvalues and the three corresponding ni are eigenvectors. The eigenvalue problem is discussed in Section 2.8.

2.8

Properties of Eigenvalues and Eigenvectors

The eigenvalue problem is governed by equation (2.30). It is the governing equation of many engineering problems. The properties of the eigenvalues and eigenvectors for a symmetric tensor σij are summarized below: 1. Eigenvalues are real. 2. Eigenvectors are real. 3. Eigenvectors are orthogonal. 4. If eigenvalues are distinct, eigenvectors can be determined uniquely.

© 2005 by Chapman & Hall/CRC Press

56

Continuum Mechanics and Plasticity 5. If two eigenvalues are identical, one eigenvector corresponding to the distinct eigenvalue is unique, other two eigenvectors lie in a plane normal to the unique eigenvector. 6. If all three eigenvalues are identical, then all directions in the space xi are eigen directions. In this case σij = λδij . 7. The principal stress components σ¯ ij and the stress components σij are related by [σ¯ ] = [Q]T [σ ][Q], where the transformation matrix [Q] is deﬁned by the eigenvectors (direction cosines between the eigenvectors and coordinate axes) and this subject is discussed in Section 2.12.

Show that if σij is symmetric, then three real roots λ1 , λ2 , λ3 exist in (2.30). This is proven by contradiction. First, we let λ be complex, that is, λ = α+iβ. For the sake of generality, let ni be complex too, that is, ni = µi + iξi . Then, α, β, µi , and ξi are real. By substitution, (2.30) becomes EXAMPLE 2.4

σij (µi + iξi ) − (α + iβ)(µj + iξj ) = 0

(a)

By equating real and imaginary parts in (a), we obtain σij µi = αµj − βξj σij ξi = βµj + αξj

(b)

Multiplying the ﬁrst equation of (b) by ξj and the second equation of (b) by µj and subtracting the two resulting equations, we get β(ξj ξj + µj µj ) = 0

(c)

Since the quantity within the parenthesis is nonnegative, we have β=0

(d)

Hence, all eigenvalues are real. EXAMPLE 2.5

Show that if σij is symmetric, then all eigenvectors of (2.30)

are real. Proof Equation (2.30) may be written as (σ11 − λ)n1 + σ21 n2 + σ31 n3 = 0 σ12 n1 + (σ22 − λ)n2 + σ32 n3 = 0 σ13 n1 + σ23 n2 + (σ33 − λ)n3 = 0

© 2005 by Chapman & Hall/CRC Press

(a)

Stress

57

Because the determinant of (a) is zero, the rank is at most two (the rank of a matrix is the dimension of the largest square submatrix with a nonvanishing determinant that is contained in the matrix); therefore, the three equations are linearly dependent and the third equation can be expressed in terms of the former two. If we delete the last equation, then the number of equation is less than the number of unknown. Hence, a real solution for n1 , n2 , and n3 always exists. If the 3 × 2 matrix has rank two, then we can solve for n1 and n2 (say) in terms of n3 , that is, n1 = N1 n3

and

n2 = N2 n3

(b)

where N1 and N2 are proportional factors determined by the two equations. But n is a unit vector and it must satisfy n21 + n22 + n23 = 1

(c)

Substituting (b) into (c), we obtain (N12 + N22 + 1)n23 = 1

(d)

which may be solved to yield n3 = (1 + N12 + N22 )−1/2

(d)

Expressions in (b) and (e) form the solution of (a). In this case, n can be found uniquely. If the rank is less than two, then n cannot be determined uniquely, the physical signiﬁcance being that there may exist more than one n such that t(n) = λn

(f)

An example is, when σ11 = σ22 , then n cannot be determined uniquely. EXAMPLE 2.6

Show that eigenvectors are mutually orthogonal.

Case 1: All λ’s are distinct (r)

In this case λ1 = λ2 = λ3 . Choose two such directions ni then (2.30) becomes (r)

(r)

(s)

(s)

σij ni − λr nj = 0 σij ni − λs nj = 0

© 2005 by Chapman & Hall/CRC Press

(s)

and ni , r = s,

(a) (b)

58

Continuum Mechanics and Plasticity (s)

Multiplying (a) by nj equations, we ﬁnd

(r)

and (b) by nj , and subtracting the two resulting (r) (s)

(λr − λs )ni ni = 0 (r)

(c)

(s)

But since λr = λs , it follows that ni ni = 0, or n(r) · n(s) = 0, for r = s. Therefore, n(r) and n(s) are mutually orthogonal. In general, we may write (r) (s)

ni ni = δrs

(d)

Case 2: Two λ’s are not distinct Assume that λ1 = λ2 and λ2 = λ3 . Choose one characteristic direction n(1) and let x1 coincide with n(1) then σij will have the form

σ11

0 0

0 σ22

σ32

0

σ23

(e)

σ33

We then examine the characteristic direction in the xi system. The characteristic equation is (for λ = λ2 )

−λ σ11 2

0 0

T (2) n1 =0 σ23 n(2) 2 (2) σ33 − λ2 n3

0

0

−λ σ22 2 σ32

(f)

(2) (2) Evidently, n1 = 0, since the ﬁrst equation of (f) is σ11 − λ2 n1 = 0 and = λ = λ . This implies that x ⊥ n(2) or n(1) ⊥ n(2) . The remaining two σ11 1 2 1 equations are (2)

(2)

(σ22 − λ2 )n2 + σ23 n3 = 0 (2)

(g)

(2)

− λ2 )n3 = 0 σ32 n2 + (σ33 (2)

(2)

The determinant of (g) vanishes for nontrivial solution of n2 and n3 . Thus, (σ − λ2 ) σ23 =0 22 σ (σ33 − λ2 ) 32

(h)

or λ22 − λ2 (σ22 + σ33 ) − σ23 σ32 + σ22 σ33 = 0

© 2005 by Chapman & Hall/CRC Press

(i)

Stress

59

The two roots are + σ σ22 1 33 )2 − 4(σ σ − σ σ ) (σ22 + σ33 ± 22 33 32 23 2 2

σ + σ33 1 − σ )2 + 4(σ σ ) (σ22 ± = 22 33 32 23 2 2

λ2,3 =

(j)

The only condition which makes λ2 and λ3 not be distinct is for the discriminant to vanish, that is, = σ32 =0 σ23

and

σ22 = σ33 = λ2

(k) (2)

(2)

Substituting these results in (g), we see that any values of n2 and n3 and, (3) (3) similarly n2 and n3 , will satisfy the characteristic equation.

2.9

Normal and Shear Components

We observed in Section 2.7 that on an inclined plane with unit normal n, the stress vector t(n) and n generally have different directions. The two vectors have the same direction only when n is the principal direction of σij . In the general case, t(n) may be decomposed into two components: one in the normal direction denoted by σ N and the other in the tangential direction denoted by σ S as shown in Figure 2.6. σ N is called the normal component and σ S the shear component of the stress vector. The normal component is expressed by σ N = t(n) · n = σji nj ni

(2.35)

and the shear component is obtained from

N

|t(n) |2 = (σ N )2 + (σ S )2

n S

FIGURE 2.6 Normal and shear stress components.

© 2005 by Chapman & Hall/CRC Press

t (n)

(2.36)

60 2.9.1

Continuum Mechanics and Plasticity Directions Along which Normal Components of σij are Maximized or Minimized

We like to ﬁnd an n such that σ N is maximized or minimized. It is noted that n is subject to the condition ni ni = 1. The method of Lagrangian multiplier denoted by λ is used, so that we maximize or minimize the expression F = σji ni nj − λni ni

(2.37)

The differentiation of (2.37) yields ∂F =0 ∂ni

or

σji nj − λni = 0

(2.38)

But, (2.38) is the condition that ni be a principal direction. Hence, the principal directions make σ N either maximum or minimum, and the max. (or min.) normal component is equal to the max. (or min.) principal value of σij .

2.9.2

The Maximum Shear Stress

We use (2.36) to obtain the expression of the shear component σ S . We ﬁnd ﬁrst from (2.8) and (2.35) the following expressions: |t(n) |2 = σji nj σki nk

(2.39)

(σ N )2 = σji ni nj σmk nk nm

(2.40)

For simplicity, we let xi coincide with principal axes, then we have only the principal stresses σ1 , σ2 , σ3 and the shear stresses are zero. In this case, (2.35) reduces to σ N = σ1 n21 + σ2 n22 + σ3 n23

(2.41)

|t(n) |2 = σ12 n21 + σ22 n22 + σ32 n23

(2.42)

and (2.39) becomes

Substituting (2.41) and (2.42) into (2.36), we obtain 2 (σ S )2 = σ12 n21 + σ22 n22 + σ32 n23 − σ1 n21 + σ2 n22 + σ3 n23

(2.43)

or (σ S )2 + [(σ1 n21 ) + (σ2 n22 ) + σ3 (1 − n21 − n22 )]2 = σ12 n21 + σ22 n22 + σ32 (1 − n21 − n22 ) (2.44)

© 2005 by Chapman & Hall/CRC Press

Stress

61

To ﬁnd the maximum σ S , we set the derivatives to zero: ∂(σ S )2 = 0, ∂n1

∂(σ S )2 =0 ∂n2

(2.45)

and we ﬁnd 2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n1 (σ1 − σ3 ) = n1 (σ12 − σ32 )

(2.46)

2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n2 (σ2 − σ3 ) = n2 (σ22 − σ32 )

(2.47)

We now discuss three cases depending on whether the principal stresses are distinct or not. Case 1:

The three principal stresses are distinct, that is, σ1 = σ2 = σ3

Common factors of (σ1 − σ3 ) and (σ2 − σ3 ) can be cancelled out from (2.46) and (2.47), respectively, so that the two equations become 2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n1 = n1 (σ1 + σ3 )

(2.48)

2[σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 )]n2 = n2 (σ2 + σ3 )

(2.49)

It follows that n1 and n2 cannot both be different from zero, because otherwise n1 can be cancelled out from (2.48) and n2 cancelled out from (2.49) to obtain the following two equations: σ 1 + σ3 =0 2

σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 ) −

(2.50)

σ 2 + σ3 =0 (2.51) 2 If these two equations are to be satisﬁed, we must have σ1 = σ2 , in contradiction with the hypothesis that σ1 = σ2 . Either n1 or n2 , therefore, must be zero. Let n1 = 0, then from (2.49) we obtain σ1 n21 + σ2 n22 + σ3 (1 − n21 − n22 ) −

2[σ2 n22 + σ3 (1 − n22 )]n2 = n2 (σ2 + σ3 )

(2.52)

which may be simpliﬁed to n22 (σ2

σ2 − σ3 − σ3 ) = 2

or

n2 = ±

1 = ± cos 45◦ 2

(2.53)

Therefore, the solution is

n1 = 0,

© 2005 by Chapman & Hall/CRC Press

1 , n2 = ± 2

n3 = ±

1 2

(2.54a)

62

Continuum Mechanics and Plasticity n

x2

45°

x3

x1

n3 = 0 n3 = 0 S

x2

S

S

n1 = 0 n2 = 0 x1 FIGURE 2.7 Maximum shear stresses.

The other two cases are

1 n1 = ± , 2 1 n1 = ± , 2

n2 = 0,

1 2

(2.54b)

n3 = 0

(2.54c)

n3 = ±

n2 = ±

1 , 2

The shear stresses σ S active in the planes of n1 = 0, n2 = 0, or n3 = 0 are shown in Figure 2.7. In the insert, we show the plane of n3 = 0. It is seen that the maximum shear stresses are making ±45◦ angles with the coordinate axes. Finally, we note that in all cases of (2.54) σS =

σ2 − σ3 2

or

σ 1 − σ3 2

or

σ 1 − σ2 2

(2.55)

which may be obtained by substituting, respectively, the planes of (2.54a,b,c) into equation (2.44) for σ S . Case 2: Two principal stresses are not distinct and we consider the case of σ2 = σ3 = σ1

© 2005 by Chapman & Hall/CRC Press

Stress

63

O

45°

x1

45°

FIGURE 2.8 Maximum shear stress in the case of σ2 = σ3 = σ1 .

This is a case of rotational symmetry about the x1 -axis. In this case, n2 is arbitrary; since σ3 = σ1 , we may use (2.48) to obtain n21 (σ1 − σ3 ) =

σ1 − σ3 2

(2.56)

We note that n1 = 0, because, if n1 = 0, then upon choosing n2 = 0, we obtain n3 = 1. Using (2.44), the case of n1 = 0 leads to σ S = 0, which is the minimum shear stress, in contradiction with the goal of ﬁnding the maximum shear stress. Simplifying (2.56), we ﬁnd n1 = ±

1 , 2

n2 = arbitrary,

n3 = arbitrary

(2.57)

In this discussion, special attention is given to the relation n21 + n22 + n23 = 1. Figure 2.8 shows a cone with generator in the x1 direction. The maximum shear stress σ S lies on the surface of the cone and its magnitude is given by σ S = 12 (σ1 − σ2 ) found on substitution of (2.57) into (2.44). Case 3: All principal stresses are equal, that is, σ1 = σ2 = σ3 = σ This is a case of hydrostatic pressure. In this case, we found from (2.43) that (σ S )2 = σ 2 (n21 + n22 + n23 ) − σ 2 (n21 + n22 + n23 )2 = 0

(2.58)

with arbitrary n1 , n2 , n3 , that is, the shear stress is zero in all directions. Finally, the following conclusion may be stated: the maximum shear stress is equal to one-half the difference between the greatest and least normal stresses and acts on the plane that bisects the angle between the directions of the largest and smallest principal stresses.

© 2005 by Chapman & Hall/CRC Press

64

2.10

Continuum Mechanics and Plasticity

Mean and Deviatoric Stresses

Any tensor of rank two can be written as (C11 + C22 + C33 ) δij Cij = αδij + Bij = 3 C13 C12 {C11 − 13 (C11 +C22 + C33 )} 1 C21 {C22 − 3 (C11 C23 + +C22 + C33 )} 1 C31 C32 {C33 − 3 (C11 +C22 + C33 )}

(2.59)

In a similar manner, the stress tensor σij can be written as σij =

(σ11 + σ22 + σ33 ) δij 3 σ13 σ12 {σ11 − 13 (σ11 +σ22 + σ33 )} σ21 {σ22 − 13 (σ11 σ23 + +σ22 + σ33 )} 1 σ31 σ32 {σ33 − 3 (σ11 +σ22 + σ33 )}

(2.60)

or σij = 13 σkk δij + σij

(2.61)

where 13 σkk is the mean stress; and σ13 σ12 {σ11 − 13 (σ11 +σ22 + σ33 )} 1 σ21 σ23 {σ22 − 3 (σ11 σij = +σ22 + σ33 )} σ31 σ32 {σ33 − 13 (σ11 +σ22 + σ33 )}

(2.62)

is the deviatoric stress tensor. Thus, the stress may be decomposed into the hydrostatic (mean stress) and deviatoric parts. This property of stress is particularly useful in the study of plasticity which is discussed further in the later chapters of this book. Plastic yielding and plastic deformation of metals are known to be independent of the hydrostatic stress but are dependent on the deviatoric stress. © 2005 by Chapman & Hall/CRC Press

Stress

2.11

65

Octahedral Shearing Stress

The concept of octahedral shearing stress is useful in plasticity as well. Consider principal stress axes. If the normal ni of a plane in this stress space makes equal angles with the three axes, there are eight directions which satisfy n21 = n22 = n23 = 13 . The eight planes associated with these eight directions are called the octahedral planes. The planes form equal angles with the principal directions and form a diamond shaped region around the zero stress point. The shearing stress σoS that acts on the octahedral planes is called the octahedral shearing stress. From (2.43), in the principal stress space, we can show that the align reduces to (σ S )2 = (σ1 − σ2 )2 n21 n22 + (σ2 − σ3 )2 n22 n23 + (σ3 − σ1 )2 n23 n21

(2.63)

If n21 = n22 = n23 = 13 , then (2.63) reduces to 9(σoS )2 = (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2

(2.64)

This is the expression for octahedral shearing stress. On the other hand, the normal component acting on the octahedral plane is given from (2.41) by σoN = 13 (σ1 + σ2 + σ3 ) = mean stress

(2.65)

We now show that the octahedral shearing stress may be expressed in terms of the stress invariants. To this end, we observe that align (2.64) can be rewritten as: 9(σoS )2 = 2(σ12 + σ22 + σ32 ) − 2(σ1 σ2 + σ2 σ3 + σ3 σ1 ) = 2[(σ1 + σ2 + σ3 )2 − 2(σ1 σ2 + σ1 σ3 + σ2 σ3 )] − 2(σ1 σ2 + σ2 σ3 + σ3 σ1 ) = 2[J12 − 2J2 ] − 2J2 = 2J12 − 6J2

(2.66)

where (2.33) was used in the principal coordinate system. It is seen that the octahedral shearing stress σoS is invariant with rotation of coordinate axes. If J1 and J2 are expressed in terms of stress components taken relative to arbitrary (x1 , x2 , x3 ) axes — not principal axes as above —, equation (2.66), on the substitution of (2.33), becomes 2 2 2 + 6σ13 + 6σ23 9(σoS )2 = (σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 + 6σ12 (2.67)

This expression forms the basis for von Mises yield criterion discussed in Chapter 6 . © 2005 by Chapman & Hall/CRC Press

66

2.12

Continuum Mechanics and Plasticity

The Stress Invariants

We would like to see now that the stress invariants deﬁned in (2.33) remain unchanged under rotation of the coordinate system. Let us assume that coordinates xi rotate into xi . The ﬁrst stress invariant is J1 = σii

(2.68)

In the coordinate system xi , we denote the components of σij by σij , then the ﬁrst invariant in the xi system is J1 = σii . Using the transformation align of the second-rank tensor (1.46), we have σii = Qri Qsi σrs = δrs σrs = σss = σii

(2.69)

Comparing (2.68) and (2.69), we ﬁnd J1 = J1

(2.70)

which shows that J1 indeed remains unchanged with rotation of the coordinate system. The third invariant is J3 = det σ = 16 eijk erst σir σjs σkt

(2.71)

In the primed coordinate system, J3 = 16 eijk erst σir σjs σkt = 16 eijk erst Qai Qbr σab Qcj Qds σcd Qek Qft σef = 16 (eijk Qai Qcj Qek )(erst Qbr Qds Qft )σab σcd σef = 16 eace ebdf σab σcd σef = J3

(2.72)

It is seen from (2.72) that J3 is an invariant. In the derivation of (2.72), we = e , which indicates that the permutation symbol is a used the relation eijk ijk third-rank isotropic tensor. The second invariant is J2 = tr cofactor σ = Mii

(2.73)

Note that we use Mij to denote the matrix of the cofactors and not the minors. We now ﬁnd the expressions for the minors. To do this, we ﬁrst expand the

© 2005 by Chapman & Hall/CRC Press

Stress

67

determinant of the stress matrix as σ11 σ12 σ13 σ21 σ22 σ23 = σ11 σ22 σ23 − σ12 σ21 σ32 σ33 σ31 σ31 σ32 σ33

σ21 σ23 + σ 13 σ33 σ31

σ22 σ32

(2.74)

We then differentiate (2.74) to obtain the minors as M11 =

∂|σ| , etc. ∂σ11

(2.75)

∂|σ| ∂σij

(2.76)

Generally, we write Mij =

Using (2.76) and (2.71), and observing the notations ∂σir = δip δrq ∂σpq

(2.77)

Mpq = 16 {epjk eqst σjs σkt + eipk erqt σir σkt + eijp ersq σir σjs }

(2.78)

We ﬁnd

The second and third terms on the right-hand side are equal to the ﬁrst term, and (2.78) may be simpliﬁed to obtain Mpq = 21 epjk eqst σjs σkt

(2.79)

Hence, we ﬁnd J2 = Mii = 12 eijk eist σjs σkt = 12 (δjs δkt − δjt δks )σjs σkt = 12 {σjj σkk − σjk σkj } = 12 {[tr σ]2 − tr(σ)2 } = 12 {J12 − tr(σ2 )}

(2.80)

Since J1 and tr(σ2 ) are invariant, we may conclude that J2 remains invariant with rotation of the coordinate system. Another representation of J2 may be obtained as follows. Using (2.79), we write Mpq σrq = 12 epjk eqst σjs σkt σrq

(2.81)

By use of the identity proven in Example 2.7, (2.81) reduces to σrq Mpq = 12 epjk erjk |σ| = δpr |σ|

© 2005 by Chapman & Hall/CRC Press

(2.82)

68

Continuum Mechanics and Plasticity

Note that the identity eirs ejrs = 2δij has been used in the derivation of (2.82). In the symbolic notation, (2.82) may be written as σ · MT = 1 · |σ|

(2.83)

If we multiply (2.83) from the left by σ−1 , we obtain MT = σ−1 |σ|

or

σ−1 =

MT |σ|

(2.84)

This indicates that the inverse of the matrix σ is the transpose of its cofactors divided by the determinant of the matrix. Using (2.84), we ﬁnd the following expression for the second invariant J2 = tr(M) = tr MT = tr(σ−1 )|σ| EXAMPLE 2.7

(2.85)

Prove the identity empq det A = eijk Aim Ajp Akq .

Proof The determinant of matrix [A] is A11 det A = A21 A31

A12 A22 A32

A13 A11 A23 = A12 A33 A13

A21 A22 A23

A31 A32 A33

(a)

An interchange of column or row of the determinant causes a sign change, and this may be expressed by A1m empq det A = A2m A3m

A1p A2p A3p

A1q A1m A2q = A1p A3q A1q

A2m A2p A2q

A3m A3p A3q

(b)

A triple product of three vectors is a1 a · (b × c) = eijk ai bj ck = b1 c1

a2 b2 c2

a3 b3 c3

(c)

When we let ai = Aim , bi = Aip , and ci = Aiq , (b) and (c) combine to give empq det A = eijk Aim Ajp Akq

© 2005 by Chapman & Hall/CRC Press

(d)

Stress

69

which proves the identity. Finally, we note that i a × b = ax b x

2.13

j ay by

k i az = j bz k

ax ay az

bx by bz

(e)

Spectral Decomposition of a Symmetric Tensor of Rank Two

In this section, we discuss a representation of a symmetric second rank tensor by its eigenvalues and eigenvectors. To this end, we derive the following relation ﬁrst (r) (r)

ni nj = δij

(r summed)

(2.86) (1)

(2)

(3)

If we denote the directions of the normalized eigenvectors ni , ni , ni by x1 , x2 , x3 , respectively, we can then make use of (1.22), which relates the base vectors of the two coordinate systems. Thus, unit vectors n(r) may be represented by (r)

n(r) = nk ek = Qkr ek

(2.87)

(r)

where nk are direction cosines of n(r) with respect to the ek system and (r)

nk = Qkr

(2.88)

The inverse of (2.87) is (r)

ek = nk n(r)

(2.89)

On the other hand, following the same procedure and using a different normalized eigenvector, we obtain (s) em = n(s) m n

(2.90)

We then form the dot product from (2.89) and (2.90) as, (r)

(r)

(r)

(s) (r) ek · em = nk n(r) · n(s) = nk n(s) m n m δrs = nk nm

(2.91)

In the derivation, we note that eigenvectors are orthogonal expressed by (r) (s)

ni ni = δrs

© 2005 by Chapman & Hall/CRC Press

(2.92)

70

Continuum Mechanics and Plasticity

Hence (2.91) reduces to (r)

nk n(r) m = δkm

(2.86)

We now use this result to derive a representation of a symmetric tensor by its eigenvalues and eigenvectors. To this end, we start with (r)

(r)

σij ni = λr nj

(r not summed)

(2.93)

(r)

Then, by multiplying both sides of (2.93) by nk and summing over r, we have (r) (r)

σij ni nk =

(r) (r)

λ r nj nk

(2.94)

r

Using (2.86), (2.94) reduces to σij =

(r) (r)

λ r ni nj

(2.95)

r

Equation (2.95) is the spectral decomposition of σij . A remark is in order. In the study of coordinate transformation in Chapter 1, we have Qki Qkj = δij

(1.25)

Qik Qjk = δij

(1.27)

where Qij is the transformation matrix between coordinate systems xi and xi . In this section, we obtain the relations (r) (s)

ni ni = δrs

(2.92)

(r) (r)

ni nj = δij

(2.86)

(r)

(r)

where ni are normalized eigenvectors. Since from (2.88) nk = Qkr , then upon substitution, (2.92) and (2.86) reduce to (1.25) and (1.27), respectively. Also, the [Q] matrix may be written as

(1)

n1

[Q] = [n(1)

n(2)

(1) n(3) ] = n2 (1)

n3

© 2005 by Chapman & Hall/CRC Press

(2)

n1

(2)

n2

(2)

n3

(3)

n1

(3) n2 (3) n3

(2.96)

Stress

2.14

71

Powers of a Tensor

Powers of a tensor σij is usually written as Square of σij = σip σpj = σ2

(2.97)

Cube of σij = σip σpq σqj = σ3 , etc.

(2.98)

For a second-rank symmetric tensor, we have the representation σij =

(r) (r)

λr ni nj

(2.99)

r

If n is a positive integer, the nth power of a tensor σ deﬁned to be the positive tensor σn whose components are σijn =

(r) (r)

λnr ni nj

(2.100)

r

This expression may be proven as follows: from (2.30), we have σij ni = λnj , so that (σij σjp )ni = λσjp nj = λ2 np

(2.101)

which shows that the square of σij has the eigenvalue of λ2 and the eigenvector of ni . The same method may continue for the third power of σij and for the general case of nth power. If n is a fraction number, then all eigenvalues need be positive. A tensor σ is said to be positive, if it has positive principal values and three linearly independent principal vectors (eigenvectors). A tensor σ is said to be positive deﬁnite if it is coefﬁcients of a positive deﬁnite quadratic form. It may be easily shown that a positive symmetric tensor is also positive deﬁnite.√Knowing a positive σ, we can ﬁnd the square root of this tensor σ1/2 = σ by ﬁrst ﬁnding the principal directions and the principal values σ1 , σ2 , and σ3 of σ; and then, in the principal space, we take the square root of the principal values so that the matrix is 1/2 σ1 0 0 1/2 σ¯ 1/2 = 0 (2.102) 0 σ2 1/2 0 0 σ3 Finally, we apply the transformation equation to obtain σ1/2 referred to the xi axes. The equation used in the axes transformation is [σ ]1/2 = [Q][σ¯ ]1/2 [Q]T

© 2005 by Chapman & Hall/CRC Press

(2.103)

72

Continuum Mechanics and Plasticity

Show that a positive symmetric tensor is also positive deﬁnite. If a tensor is positive, its eigenvalues are all positive, that is, λ1 > 0, λ2 > 0, λ3 > 0. In the principal coordinate system, the expression of quadratic form σij ni nj is λ1 n21 + λ2 n22 + λ3 n23 . If λ1 > 0, λ2 > 0, and λ3 > 0, then λ1 n21 + λ2 n22 + λ3 n23 > 0, which shows that the quadratic form is positive deﬁnite. On the other hand, it may be shown that a positive deﬁnite (symmetric) tensor is positive. To this end, we consider σij ni nj > 0. In the principal coordinate system, the quadratic form is reduced to

EXAMPLE 2.8

λ1 n21 + λ2 n22 + λ3 n23 > 0

(a)

We note that ni is one of the eigenvectors, so that if n1 = 0 and n2 = n3 = 0, (a) reduces to λ1 n21 > 0, which leads to λ1 > 0. Similarly, λ2 > 0, λ3 > 0 and, therefore, σ is a positive tensor.

2.15

Cayley–Hamilton Theorem

The aim of this section is to indicate that, by use of the Cayley–Hamilton theorem, a high-order matrix polynomial may be reduced to a lower order one. In this manner, a nonlinear expression can be reduced to an expression with second-order term as its highest power term, and thus simplifying the mathematics involved. According to this theorem, a square matrix satisﬁes its own characteristic align, that is, σ3 − J1 σ2 + J2 σ − J3 δ = 0

(2.104)

In the principal space, (2.104) is written as λ3r − J1 λ2r + J2 λr − J3 = 0

where r = 1, 2, 3

(2.105)

and, in the matrix form, (2.105) is

σ13 0 0

0 σ23 0

2 0 σ1 0 − J1 0 σ33 0

0 σ22 0

0 σ1 0 + J2 0 0 σ32

0 σ2 0

0 1 0 − J3 0 σ3 0

0 1 0

0 0 = 0 1 (2.106)

where σ1 , σ2 , σ3 are the three principal values. In the index notation, (2.104) is written as σim σmn σnj − J1 σim σmj + J2 σij − J3 σij = 0

© 2005 by Chapman & Hall/CRC Press

(2.107)

Stress

73

This equation is valid in the general case and not necessarily in the principal directions. But the formal proof is lengthy and is to be found in a textbook on linear algebra. The proof will not be discussed here. We show next that the expression of J2 may be found by using this theorem. Multiplying (2.104) by σ−1 , we ﬁnd σ2 − J1 σ + J2 δJ3 σ−1 = 0

(2.108)

Taking the trace of all terms in the above equation, we obtain tr σ2 − J12 + 3J2 − J3 tr(σ−1 ) = 0

(2.109)

Since the last term is, from (2.85), −J2 , (2.109) may be solved to yield J2 = 12 (J12 − tr σ2 )

(2.110)

This expression is similar to that derived earlier in (2.80). By use of the Cayley–Hamilton theorem, we can reduce the nth (positive integer) power of a matrix to a linear combination of the second, ﬁrst, and zeroth powers. For example, if we multiply (2.104) by σ, we obtain σ 4 − J 1 σ3 + J 2 σ2 − J 3 σ = 0

(2.111)

By applying (2.104) again, (2.111) becomes σ4 − J1 {J1 σ2 − J2 σ + J3 δ} + J2 σ2 − J3 σ = 0

(2.112)

σ4 = σ2 {J12 − J2 } − σ{J1 J2 − J3 } + J1 J3 δ

(2.113)

which leads to

It is seen that σ4 may be expressed in terms of σ2 , σ, and δ. It is important to note that the coefﬁcients of the second, ﬁrst, and zeroth-power terms are functions of the invariants of σ. In a similar manner, a matrix of any power higher than two may be expressed in terms of σ2 , σ, and δ.

References 1. Malvern, L.E., Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Englewood Cliffs, NJ, 1969. 2. Prager, W., Introduction to Mechanics of Continua, Ginn, Boston, MA, 1961. 3. Eringen, A.C., Mechanics of Continua, Wiley, New York, 1967.

© 2005 by Chapman & Hall/CRC Press

74

Continuum Mechanics and Plasticity 4. Fung, Y.C., Foundations of Solid Mechanics, Prentice-Hall, Englewood Cliffs, NJ, 1965. 5. Truesdell, C. and Toupin, R., The Classical Field Theories, in Handbuch der Physik, Vol. III/1, S. Flugge, Ed., Springer-Verlag, Berlin, 1960. 6. Sokolnikoff, I.S., Mathematical Theory of Elasticity, McGraw-Hill, New York, 1956.

Problems (1) A specimen used for uniaxial tensile testing of material has a middle section (the gauge section) of reduced cross-section. The stress is uniformly distributed within this section. You may consider this section as a circular cylinder. When the specimen is pulled, what stress boundary conditions (stress vectors) apply in the middle section of the specimen? (2) An inﬁnitesimal material element is subjected to hydrostatic pressure p as shown in Figure 2.9. Determine the stress vector acting on surface a–a of the element.

p

a⬘ p

p a

p

FIGURE 2.9

(3) The bar shown in Figure 2.10 has a cross-sectional area A and is subjected to the axial load P. Determine the stress vector acting on the inclined surface a–a .

a⬘ P

P a

FIGURE 2.10

© 2005 by Chapman & Hall/CRC Press

Stress

75

(4) The state of stress for the inﬁnitesimal tetrahedron OABC shown in Figure 2.11 is

20 [σ ] = −60 40

−60 0 80

40 80 MPa −20

Determine the stress vector acting on the inclined plane ABC. x3

C(0,0,1)

B(0,1,0)

O

x2

A(2,0,0) x1 FIGURE 2.11

(5) Let the components of the stress tensor at point P be given in matrix form by

21 [σ ] = −63 42

−63 0 84

42 84 MPa −21

Determine the stress vector on a plane passing through P, parallel to the x3 -axis and making a 30◦ counterclockwise angle from the x1 -axis. (6) If the components of the stress tensor is given by

1 σij = 0.5 0

0.5 −1 −0.2

0 −0.2 MPa 0

determine √ the stress vector acting on a surface whose normal is n = 0.2e1 + 0.3e2 + 0.87e3 . What are the normal and shear components acting on the surface? (7) In the principal stress space, determine the expression of stress vector (in terms of stress components) acting on the octahedral plane in the ﬁrst quadrant of the stress space.

© 2005 by Chapman & Hall/CRC Press

76

Continuum Mechanics and Plasticity (8) Stress is a second-rank tensor. If the stress components referring to the xi coordinate system are

6 [σij ] = 2 0

2 −1 0

0 0 MPa 1

ﬁnd the stress components of the same tensor with respect to the xi system if x3 = x3 and x1 is making a 30◦ angle counterclockwise with the x1 -axis. (9) The stress tensor at point P has the following components with respect to the xi coordinate system

20 [σ ] = 0 −10

0 8 0

−10 0 MPa 24

Referring to Figure 2.12, if the x1 -axis makes equal angles θ with the three xi axes and the x2 -axis lies in the x1 x2 plane, determine the components of the stress tensor referred to the right-handed xi coordinate system. x3

x⬘1 P

x2

x1

x⬘2

FIGURE 2.12

(10) The stress tensor is σij = α(νi νj + νj νi ), where α is a scalar and ν and ν are unit vectors. Determine the principal stresses and axes. (Hint: to simplify the computation, choose the x1 -axis parallel to ν and the x3 -axis normal to ν and ν ).

© 2005 by Chapman & Hall/CRC Press

Stress

77

(11) Let t1 , t2 , and t3 be the stress vectors acting on surface elements that are normal to the coordinate axes. Show that the sum of the squares of the magnitudes of these vectors is independent of the orientation of the coordinate axes. (12) Consider the following stress distribution

ax2 σ= b 0

b 0 0

0 0 0

where a and b are constants. Determine and sketch the distribution of the stress vector acting on the square in the x1 = 0 plane, with vertices located at (0, 1, 1), (0, −1, 1), (0, 1, −1), (0, −1, −1). (13) A block of unit thickness is subjected to forces shown in Figure 2.13. The area of face (1) is A1 and the area of face (2) is A2 . (a) Determine the stress vectors acting on these two surfaces; (b) ﬁnd the conditions which must be satisﬁed by the forces and areas for the block to be in equilibrium; (c) if the stress is uniformly distributed in the block, determine the components of the stress tensor; (d) if principal stresses apply on the material element shown with orientation speciﬁed by φ, ﬁnd the second stress invariant J2 at this conﬁguration. x2 F4

Face 2

F3 F2 F1

x1

Face 1

FIGURE 2.13

(14) For the state of stress given by

10 [σ ] = 30 −50

30 0 0

−50 0 MPa 0

ﬁnd the components of the deviatoric stress σij and determine the principal invariants of the deviatoric stress.

© 2005 by Chapman & Hall/CRC Press

78

Continuum Mechanics and Plasticity

(15) Cut out a tetrahedron of inﬁnitesimal size from a body. The normal of the inclined face makes equal angles with the three coordinate axes. Find the force that must be applied on the inclined face so that it will produce a state of stress given by the following matrix

30 [σ ] = −10 20

−10 0 10

20 10 MPa 10

For equilibrium, what forces must be applied to the faces normal to the coordinate axes? (16) The second invariant of the deviatoric part of σ is denoted by J2 . Show that . Note that the differentiation is taken with respect to σ and ∂J2 /∂σpq = −σqp pq not σpq . (17) If [Q] = [n(1) n(2) n(3) ] and [Q]T [Q] = [δ], show that by use of (σij − λδij )ni = 0, it may be shown that

λ1 [Q]T [σ ][Q] = 0 0

0 λ2 0

0 0 λ3

that is, [σ ] may be diagonalized by use of [Q]. Show also that tr QT σQ = λ1 + λ2 + λ3 . (18) A stress ﬁeld is given by the matrix

(1 − x22 )x1

0

(1 − x22 )x1

− 12 (x22 − 4x2 )

0

0

0

(4 − x12 )x2

[σ ] =

(1 + x12 )x2 + 12 x22

Find the expression for the second invariant of the deviatoric stress. (19) If J1 , J2 , and J3 denote the principal invariants of the stress tensor σij and J1 , J2 , and J3 denote the principal invariants of the deviatoric stress σij , show that J1 = J1 + 3σm = 3σm 1 J2 = J2 + J12 3 2 1 3 J3 = J3 + J1 J2 + J 9 27 1

© 2005 by Chapman & Hall/CRC Press

3 Motion and Deformation

3.1

Introduction

In this chapter, we consider the motion of a body and, in particular, we concentrate on the study of deformation and the rate of change of a material element on or within the body. We assume the reader has familiarized himself with the concepts of strain and strain-rate in the study of elementary mechanics of deformable bodies. Strain describes the change in the geometry of an element in a body. But strain and strain-rate need to be deﬁned. There are several measures of strain that people use. Deformation is a more general terminology to use than strain in describing the geometrical change of a material element (see [1–4] for further reading). The particles of the body may occupy various positions in a threedimensional space. The complete speciﬁcation of the positions of the particles of a body is called the conﬁguration of a body. The conﬁguration of the body at the reference time (or initial or undeformed state) and at the current time (or deformed state) is the reference conﬁguration denoted by R0 , and the current conﬁguration denoted by Rt , respectively. To ﬁx the concept of deformation, let us consider a material point P within a neighborhood N0 at the reference conﬁguration. Referred to in Figure 3.1, point P moves to point p within a neighborhood Nt at the current conﬁguration due to load applied to the body. The concept of deformation may be understood by taking two photographs of the material element, one at the reference conﬁguration and the other at the current conﬁguration. We then compare and characterize the size and shape of the material element in the two photographs. The change in the size and shape of the material element is called the deformation of the material element and it indicates its need to be quantiﬁed. We also observe that time is not a factor in the study of deformation. To describe the two conﬁgurations, a material (Lagrangian) coordinate system, denoted by XR , and a spatial (Eulerian) coordinate system, denoted by xi , is introduced. The position of the material point P at the reference conﬁguration is speciﬁed by the material coordinates XR and that of p at the current conﬁguration is speciﬁed by the spatial coordinates xi . For convenience, the undeformed conﬁguration of a material element is often chosen as the 79

© 2005 by Chapman & Hall/CRC Press

80

Continuum Mechanics and Plasticity

p(xi) Nt

Rt

P(XR) N0

R0 x3

X3

eR

O

ei

x2

X2

O X1

x1

FIGURE 3.1 Reference and current conﬁgurations.

reference conﬁguration. But, any other conﬁguration may also be chosen as the reference conﬁguration, if needed. Once a reference conﬁguration has been chosen, all the material points of a body can be described by the material coordinates XR . In the general case, the axes of XR and xi do not have the same origin and orientation as shown in Figure 3.1. But, in many cases, it is convenient to select the two coordinate systems such that they have the same origin and orientation. This selection leads to simplicity and is used in most of the topics discussed in this book. Motion may be viewed as a family of deformations continuously varying in time, and the deformations between two conﬁgurations have been discussed in the previous paragraph. When a continuum is in motion, physical quantities associated with a material element of the body (such as density ρ, velocity v, etc.) change with location and time. The motion of a continuous body may be described in two ways: material and spatial descriptions. The material description has been used mostly in solid mechanics and the spatial description in ﬂuid mechanics. Some recent works have used a mixed description. We now discuss the two descriptions in the light of time-dependent motions.

3.2 3.2.1

Material and Spatial Descriptions Material Description

The material description is also known as the Lagrangian description. In this description, a material element is followed. The observer sits on top of the body and moves with the body. He observes changes in the physical

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

81

quantities of the body as functions of the material element identiﬁed by the material coordinates XR and time t. Therefore, we write ρ = ρ(XR , t),

3.2.2

v = v(XR , t), etc.

(3.1)

Spatial Description

The spatial description is also known as the Eulerian description. Here, the observer observes the changes in physical quantities at a ﬁxed location in the laboratory. Hence, the quantities are described in terms of the location in space denoted by the spatial coordinates xi and time t. In effect, we describe and measure the quantities at a ﬁxed location and they are functions of time. Spatial positions are occupied by different particles at different times. Therefore, the spatial description does not provide direct information related to changes in the properties of the material element as the body moves. In this description, we write ρ = ρ(xi , t),

v = v(xi , t), etc.

(3.2)

If we know the motion of the body, then the two descriptions are related and are equivalent. One description can be obtained from the other. The correlation between the two descriptions is now discussed. During the motion of the body, particle P with position vector X moves to point p with position vector x and the displacement is u=x−X

(3.3)

In the material description, the above equation is written as u(X, t) = x(X, t) − X

(3.4)

and, in the spatial description, it is written as u(x, t) = x − X(x, t)

(3.5)

The velocity v of a particle is the rate of change of its displacement, and, in the material description, it is written as v(X, t) =

∂[x(X, t) − X] ∂x(X, t) Dx ∂u(X, t) = = ≡ ∂t ∂t ∂t Dt

(3.6)

where D/Dt is called the material derivative. The motion of the particle is followed and material coordinate X is ﬁxed during this motion. In the index

© 2005 by Chapman & Hall/CRC Press

82

Continuum Mechanics and Plasticity

notation, (3.6) is written as vi (XR , t) =

∂xi (XR , t) ∂t

(3.7)

Note that the expression in (3.7) is different from the spatial description, which is vi (xj , t) for the particle velocity. The relationship between the two descriptions is illustrated in Example 3.1. EXAMPLE 3.1

A body undergoes the motion deﬁned by x1 = X1 (1 + a1 t + a2 t2 ),

x2 = X2 ,

x3 = X3

(a)

where a1 and a2 are constants. Find the displacement and velocity in both the material and spatial descriptions. Solution In the material description, we have from (3.4), ui (XR , t) = xi (XR , t) − Xi

(b)

When equation (a) is substituted into (b), we obtain u1 = x1 − X1 = X1 (a1 t + a2 t2 ) u2 = x2 − X2 = 0

(c)

u3 = x3 − X3 = 0 Equations (c) represent the components of the displacement vector at time t in the material description. To obtain the displacement in the spatial description, we substitute for X1 by use of (a) and obtain u1 =

x1 (a1 t + a2 t2 ) , 1 + a1 t + a2 t 2

u2 = 0,

u3 = 0

(d)

Equations (d) are the displacement components in the spatial description. For the velocity, we differentiate (a) with respect to t, keeping XR ﬁxed, to obtain v1 = X1 (a1 + 2a2 t),

v2 = 0,

v3 = 0

(e)

Equation (e) is in the material description and, for the spatial description, we eliminate X1 from (e) to obtain v1 =

x1 (a1 + 2a2 t) , 1 + a1 t + a2 t 2

v2 = 0,

We see that (f) is in the spatial description.

© 2005 by Chapman & Hall/CRC Press

v3 = 0

(f)

Motion and Deformation

3.3

83

Description of Deformation

We refer to the motion of a continuum when a body is undergoing change in geometry due to applied forces. The motion is generally described by the set of equations xi = xi (XR , t)

i = 1, 2, 3

(3.8)

These equations describe the change in position of a generic particle P with coordinates XR into p with coordinates xi . The functional relationship in (3.8) is generally nonlinear and its dependence on time t is discussed later in this chapter associated with material rate of change and rate of deformation. In this section, we study the deformation, that is, we set t to a constant time in (3.8). It is assumed that the mapping between XR and xi is one-to-one and onto; that is, for every particle in R0 there corresponds one point only in Rt and to every point in Rt there corresponds one particle only in R0 . Thus, the relation can be inverted to yield XR = XR (xi , t)

(3.9)

This assumption automatically satisﬁes the physical principle of conservation of mass and is a property of continuity. Motion described by (3.8) is the material description, where the variables are the material coordinates XR and time t; motion described by (3.9) is a spatial description, where the variables are xi and t. In this section, we study the deformation that has taken place at a speciﬁed time t. A special case of (3.8) is that xi is a linear function of XR such that xi = QiR (t)XR

(3.10)

If QiR is an orthogonal tensor, then QiR rotates vector XR into vector xi , which has been discussed in Section 1.6.2.

3.4

Deformation of a Neighborhood

Consider the deformation of a small material vector dX, which maps into vector dx in the deformed conﬁguration. Vector dX connects two neighboring points in neighborhood N0 and it may be considered as a line element between the two points. Due to deformation, the initial line element dX deforms into the current (deformed) line element dx and they are related by dx =

© 2005 by Chapman & Hall/CRC Press

∂x · dX = F · dX ∂X

(3.11)

84

Continuum Mechanics and Plasticity

where F = ∂x/∂X is called the deformation gradient, which plays an important role in modern continuum mechanics. In the component form, the deformation gradient F is written as F=

∂xi ei ⊗ eR = FiR ei ⊗ eR ∂XR

(3.12)

where eR and ei are base vectors of the material and special coordinate systems, respectively. Substituting (3.12) into (3.11), we have dxi ei =

∂xi ∂xi ∂xi ei ⊗ eR · dXS eS = dXS ei δRS = dXR ei ∂XR ∂XR ∂XR

(3.13)

Thus, the component form is obtained as dxi =

∂xi dXR = FiR dXR ∂XR

(3.14)

Note that the derivative ∂xi /∂XR is evaluated at point P and is common to all vectors dXR emanated from P within the neighborhood N0 . (In the mathematical expression f (x) = f0 + f (0)x + O(x2 ), the ﬁrst derivative f (0) is independent of x.) In the matrix form, (3.14) is written as x1,1 dx1 dx2 = x2,1 dx3 x3,1

x1,2 x2,2 x3,2

dX1 x1,3 x2,3 dX2 x3,3 dX3

(3.15)

and the Jacobian of the transformation is ∂xi J = ∂X

R

= det[F] = 0

(3.16)

If both xi and XR systems are right (or left) handed for all t, then det[F] > 0. This means that an inﬁnitesimal volume element (with ﬁnite value) cannot be deformed into a point. The volume change is discussed further later in this chapter. Some simple examples of ﬁnite deformation is considered in the concluding part of this section. We use ﬁnite versus inﬁnitesimal to distinguish large deformation from small deformation. In this chapter, most of our discussions are aimed at ﬁnite deformations. But, at the end of the chapter, we consider inﬁnitesimal deformation as a special case.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation 3.4.1

85

Homogeneous Deformations

Deformations of the form xi = ci + AiR XR

(3.17)

are homogeneous deformations. In (3.17), ci and AiR are constants or functions of time, but not functions of position XR . In this case, the deformation is the same for all points throughout the body being studied. We note that (3.17) is a linear form of the deformation equation (3.8). 3.4.1.1 Uniform extensions We consider a cube undergoing extensions in all three directions, so that x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

(3.18)

where λi specify the deformation and are constants or functions of time t. Note that (3.18) is a special case of (3.17). The deformation gradient of (3.18) may be found from (3.12) as

λ1 [F] = 0 0

0 λ2 0

0 0 λ3

(3.19)

If λ1 = λ2 = λ3 , the cube undergoes a uniform expansion or contraction in all directions and is referred to as a uniform dilatation. The volume of a material element in the cube was initially dV = dX1 dX2 dX3 and is now dv = dx1 dx2 dx3 = λ1 λ2 λ3 dX1 dX2 dX3 . Therefore, when there is no volume change, we write λ1 λ2 λ3 = 1. The volume change of an element is discussed further in a later section. In the case of an extension in the x1 direction of a long bar of uniform cross-section, λ2 = λ3 . When λ1 > 1, that is, stretching, it is usually observed that λ2 < 1. Note that λi > 0, because the length of a line element cannot become negative. 3.4.1.2 Simple shear In this deformation, parallel planes are displaced relative to each other with the distance between the planes unchanged. A square element is deformed into a parallelepiped. Thus, particle P with position vector X moves to p with position vector x as shown in Figure 3.2. The following set of equations describes a simple shear deformation: x1 = X1 + X2 tan γ ,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(3.20)

86

Continuum Mechanics and Plasticity x2

p

P

X x

x1

O FIGURE 3.2 Simple shear deformation.

where angle γ measures the amount of shear; the X2 = constant planes are the shear planes; and X1 is the shear direction. The deformation gradient of simple shear is found from (3.20) as

1 [F] = 0 0

3.4.2

tan γ 1 0

0 0 1

(3.21)

Nonhomogeneous Deformations

Equation (3.17) of homogeneous deformation leads to a deformation gradient F, which is not a function of position XR . Examples are (3.19) and (3.21). In the case of nonhomogeneous deformations, F is a function of position, that is, the deformation will be different from point to point. We consider torsion of a circular cylinder as an example of nonhomogeneous deformation. Referring to Figure 3.3, we choose the X3 axis to coincide with the axis of the cylinder. If the cylinder is twisted about the X3 axis, then plane cross-sections remain plane but are rotated rigidly through an angle τ X3 about the X3 axis. It is seen that this angle is proportional to the coordinate X3 , that is, the angle is zero at the base of the cylinder where X3 = 0 and increases its value as X3 increases. The quantity τ denotes the angle of twist per unit length and is a constant if the torque is applied at the two ends of the cylinder. In order to ﬁnd the equations of transformation that govern the deformation due to torsion, let us consider a typical cross-section shown in the insert of Figure 3.3. In the action of torsion, particle P(X1 , X2 , X3 ) with a radial distance R from the center of the circular section is rotated into p(x1 , x2 , x3 ), also with a radial distance R. At the initial position P, we have X1 = R cos α,

© 2005 by Chapman & Hall/CRC Press

X2 = R sin α,

1/2 with R = X12 + X22

(3.22)

Motion and Deformation

87

X3 R X3 p

X3

X2

P X1

Ο

X2

X1 FIGURE 3.3 Torsion of a circular cylinder.

After deformation at p, we write x1 = R cos(τ X3 + α),

x2 = R sin(τ X3 + α)

(3.23)

We then expand the cosine and sine functions in (3.23) and, by use of (3.22), obtain x1 = X1 cos τ X3 − X2 sin τ X3 ,

x2 = X1 sin τ X3 + X2 cos τ X3 ,

x2 = X3 (3.24)

Note that the equation in the 3-direction has been added due to the fact that the cross-section at a distance X3 from the base of the cylinder has merely undergone a rigid-body rotation. We conclude that (3.24) are the transformation equations that describe the deformation of a circular cylinder subjected to torsion. Differentiating (3.24), the deformation gradient F is found as

cos τ X3

[F] = sin τ X3 0

− sin τ X3 cos τ X3 0

−τ (X1 sin τ X3 + X2 cos τ X3 ) τ (X1 cos τ X3 − X2 sin τ X3 ) 1

(3.25)

It is seen that the deformation gradient depends on position for this nonhomogeneous problem. We have assumed in this discussion that the cylinder is undergoing a ﬁxed-end torsion. In this case, there is no length change in the cylinder and the radius R of the cylinder does not change. The free-end torsion is discussed in a later chapter related to plastic deformation.

© 2005 by Chapman & Hall/CRC Press

88

3.5

Continuum Mechanics and Plasticity

The Deformation Gradient

The deformation gradient plays an important role in modern continuum mechanics and is discussed in detail here. The deformation gradient F is a second-rank tensor; according to the polar decomposition theorem, a secondrank tensor can be expressed as a product of a positive symmetric tensor with an orthogonal tensor. There are two decompositions: the right and the left decompositions. They are expressed as F =R·U

right decomposition

(3.26)

F =V·R

left decomposition

(3.27)

where U and V are positive symmetric tensors, and R is an orthogonal tensor.

3.5.1

The Polar Decomposition Theorem

This theorem applies to any second-rank tensor, and there are the right and left decompositions as shown in (3.26) and (3.27). In this subsection, we consider a second-rank tensor Fij . This tensor acquires the physical meaning of deformation gradient in later sections. We now derive the right decomposition and consider tensor Fij transforms vector vi into vector vi ; the relation is vi = Fij vj

(3.28)

If the transformation (or mapping) is one-to-one, then the magnitude of vector vi is T |v |2 = vi vi = Fij Fik vj vk = Fki Fij vj vk > 0

(3.29)

T F is a posThis is a positive deﬁnite quadratic form. The coefﬁcient Ckj = Fki ij itive deﬁnite tensor. It is obvious that Ckj = Cjk . Since C is positive, a tensor √ U ≡ C is well deﬁned and it has the same eigenvectors as C. Thus,

U2 = FT · F ≡ C

(3.30)

Since C is symmetric, U is symmetric too. Now let R ≡ F · U−1 and it is seen that if we deﬁne R in this manner, then R is an orthogonal tensor. Using this expression for R, we have RT · R = (F · U−1 )T · (F · U−1 ) = (U−1 )T · FT · F · U−1 = U−1 · FT · F · U−1 = U−1 · C · U−1 = 1

© 2005 by Chapman & Hall/CRC Press

(3.31)

Motion and Deformation

89

Equation (3.30) is used in the last identity of (3.31). We see from (3.31) that R is an orthogonal tensor. In the above derivation, we also used the symmetric property of U and the relation (U−1 )T = U−1 . We have thus shown that F = R · U in which R is orthogonal and U is positive and symmetric. Following an analogous procedure, we derive the left decomposition. The resulting equations are F = V · R∗

and V2 = F · FT ≡ B

(3.32)

We now show that the orthogonal tensor R∗ of the left decomposition in the ﬁrst equation of (3.32) is indeed equal to the orthogonal tensor R of the right decomposition. From (3.32), we write F = V · R∗ = R∗ · (R∗T · V · R∗ )

(3.33)

and view the last expression in (3.33) as the right decomposition. Since the right decomposition is unique (see Example 3.2), we compare (3.33) with (3.26) to obtain R∗ = R

and U = RT · V · R

(3.34)

We see that U and V are related through equation (3.34). This relation can also be written as V = R · U · RT

(3.35)

Tensor B deﬁned in (3.32) can be shown to be related to tensor C deﬁned in (3.30). From the deﬁnition of B, we have B = F · FT = R · U · UT · R T = R · U2 · R T = R · C · R T

(3.36)

Hence, B = R · C · RT EXAMPLE 3.2

or

C = RT · B · R

(3.37)

Show that the right decomposition (3.26) is unique.

Proof Assume two decompositions exist: ¯ ·U ¯ F =R·U =R

(a)

¯T·R ¯T FT = UT · R T = U

(b)

Then, the transpose of (a) is

© 2005 by Chapman & Hall/CRC Press

90

Continuum Mechanics and Plasticity

Multiplying (a) and (b), we get ¯T·R ¯T ·R ¯ ·U ¯ FT · F = UT · R T · R · U = U ¯T·U ¯T = UT · U = U ¯2 = U2 = U

(c)

¯ and is positive. The uniqueness of R From (c), we conclude that U = U ¯ we conclude that R = R. ¯ follows from (a). Since U = U,

3.5.2

Polar Decompositions of the Deformation Gradient

If the tensor F in the previous subsection is assigned a physical meaning, then all the derived quantities have physical signiﬁcance. The polar decompositions of the deformation gradient F are F =R·U =V·R

FiR = RiS USR = Vij RjR

(3.38)

where F = deformation gradient = FiR ei ⊗ eR

(3.39a)

U = right stretch tensor = URS eR ⊗ eS

(3.39b)

V = left stretch tensor = Vij ei ⊗ ej

(3.39c)

R = rotation tensor (orthogonal tensor) = RiR ei ⊗ eR

(3.39d)

T

2

C = F · F = U = right Cauchy–Green deformation tensor, CRS = (∂xi /∂XR )(∂xi /∂XS )

(3.40)

B = F · FT = V2 = left Cauchy–Green deformation tensor, Bij = (∂xi /∂XR )(∂xj /∂XR )

(3.41)

where eR and ei are base vectors for the material and spatial system, respectively. We now discuss the physical meaning of the polar decompositions. The deformation gradient F deforms an element in two parts. In the right decomposition, the element is ﬁrst purely deformed to a quantity U. A rotation R then follows the deformation. This rotation represents the rotation of the principal axis of the stretch tensor U, which will be illustrated by Example 3.3. The above statement may be understood by applying F to a line element dX. Thus, dx = F · dX = R · (U · dX)

© 2005 by Chapman & Hall/CRC Press

(3.42)

Motion and Deformation

91

In the left decomposition, the element is ﬁrst rotated through R and then deformed by V. This statement may be veriﬁed by dx = F · dX = V · (R · dX)

(3.43)

The two modes of decomposition are fully equivalent. We obtain the same ﬁnal result. EXAMPLE 3.3

Consider a simple shear problem deﬁned by

x1 = X1 + kX2 ,

x2 = X2 ,

2 where k = √ 3

x3 = X3

(a)

(a) Find F, U, V, and R. (b) Use the right decomposition to draw ﬁgures showing the deformed state of the initially rectangular element at each stage of deformation. (c) Use the left decomposition to draw ﬁgures showing the deformed state of the initially rectangular element at each stage of deformation. (d) Study the deformation of a diagonal of the initially rectangular element. (e) Study the deformation of a circle in the initially rectangular element. Solution (a) Using (a), (3.39), and (3.40), we obtain 1 k 0 1 [F] = 0 1 0 , [F]T = k 0 0 1 0

0 0 1 0 , 0 1

1 1 k 0 T 2 2 [C] = [F] [F] = k (k + 1) 0 = √ 3 0 0 1 0

2 √ 3 7 3 0

(b)

0 0 1

(c)

To determine the principal values and directions of [C], we consider the characteristic equation

1 − λ 2 √ 3 0

© 2005 by Chapman & Hall/CRC Press

2 0 √ 3 n1 7 n2 = 0 −λ 0 3 n3 0 1−λ

(d)

92

Continuum Mechanics and Plasticity

By setting the determinant of the coefﬁcient matrix to 0, we obtain λ(i) = 3, 13 , 1. The corresponding eigenvectors are found to be

T nu(1)

=

√ 3 1 , ,0 , 2 2

3 1 , ,0 , = − 2 2

√

T nu(2)

nu(3) = [0, 0, 1] T

(e)

with the following transformation matrix between xi and xi (see (2.96)):

[Qu ] = nu(1)

(2)

nu

1 2

√ (3) nu = 3 2 0

√ − 3 2

0 0 1

1 2 0

(f)

These eigenvectors are shown in Figure 3.4 with φ = 60◦ . Referring to the principal axes xi , tensors C and U have components

3

[C ] = 0 0

0 0

0 1 3 0

√ 3 √ C = 0 and [U ] =

1

0

0 1 √ 3

0

0

1

0

(g)

It may also be veriﬁed that C is obtainable from the following transformation:

√ 3 1 2 2 √ T [C ] = [Qu ][C][Qu ] = − 3 1 2 2 0 0 3 0 0 1 = 0 0 3 0 0 1

0 1 2 √ 0 3 0 1

2 √ 3 7 3 0

1 0 2 √ 3 0 2 1 0

√ − 3 2 1 2 0

0 0 1

(h)

In addition, U can be determined by the following transformation: √ 3 2 [U] = [Qu ][U ][QuT ] = 1 2 0

© 2005 by Chapman & Hall/CRC Press

1 2 5 √

2 3 0

0 0 1

(i)

Motion and Deformation

93 2

n(1) = (cos , sin , 0)

n(2) = (–sin , cos , 0)

1

O FIGURE 3.4 Eigenvectors of C in simple shear deformation.

Since det[U] = 1, we ﬁnd

5 2√3 (cof[U])T [U −1 ] = = −1 det[U] 2 0

−1 2 √ 3 2 0

0 0 1

(j)

and [R] to be √ 3 2 [R] = [F][U −1 ] = −1 2 0

1 2 √ 3 2 0

0 0

(k)

1

The matrix in (k) describes a clockwise rotation of 30◦ of the continuum about the x3 axis. Note that √ √ 3 3 −1 1 0 0 1 0 0 2 2 2 2 √ √ T [R][R] = −1 (m) 1 = 0 1 0 3 3 0 0 0 0 1 2 2 2 2 0 0 1 0 0 1 which shows that RT = R−1 and R is therefore an orthogonal tensor. On the other hand, we may ﬁnd from the left decomposition 5 √ 2 3 [V] = [F][R−1 ] = 1 2 0

© 2005 by Chapman & Hall/CRC Press

1 2 √ 3 2 0

0

0 1

(n)

94

Continuum Mechanics and Plasticity

It may be easily shown that √ 3 [V ] = [U ] = 0 0

0 1 √ 3 0

0

0

(o)

1

and the principal directions of V are T n(1) v

√ 3 1 , , 0 , = 2 2

√ 3 1 , 0 , = − , 2 2

T n(2) v

n(3) = [0, 0, 1] v T

(p) with the transformation matrix given by (2) [Qv ] = n(1) nv v

(3)

(q)

nv

By use of (3.35), R rotates U into V. It also rotates vectors nu into nv . Putting all eigenvectors together in a matrix form, we may write √ √ √ 1 1 − 3 3 3 1 0 0 − 0 2 2 2 2 2 2 √ √ √ [Qv ] = [R][Qu ] = −1 3 = 1 3 3 1 0 0 0 2 2 2 2 2 2 0

0

1

0

0

1

0

0

1 (r)

All nu vectors that form Qu are rotated clockwise at a 30◦ angle into the nv vectors. This rotation is shown in Figure 3.5. (b) Consider a square element ABCD with unit side length, as shown in Figure 3.6. Using (3.42), the square ABCD is ﬁrst deformed by U into A B C D , which is subsequently rotated by R into A B C D . Thus, in the application n(2) v

2

nu(1)

nu(2)

n (1) v 30° 60° O

FIGURE 3.5 Rotation of nu into nv .

© 2005 by Chapman & Hall/CRC Press

1

Motion and Deformation

95 nu(1)

x2 C⬘ P⬘ B⬘ R B

C

P

B⬙

n(1) v P⬙

C⬙

D⬘ 30° A

60° D

x1

FIGURE 3.6 Right polar decomposition.

of U, line element AB is deformed into A’B’, AC into A C , etc. The deformed line elements are √ 1 1 3 0 2 2 2 0 √ 5 AB = 1 (s1) 5 3 1 = 0 √ 6 0 2 2 3 0 0 0 1 √ 3 1 0 1 1 2 2 √ 3 √ 5 AP = 1 (s2) = 3 0 1 √ 2 0 2 3 0 0 0 1 √ √ 1+ 3 1 3 0 2 2 2 1 √ 5 AC = 1 (s3) 1 = 3 + 5 3 0 √ 0 2 2 3 6 0 0 1 0 √ √ 3 1 3 0 2 2 1 2 5 A D = 1 (s4) 0 = 1 0 √ 0 2 2 2 3 0 0 1 0

© 2005 by Chapman & Hall/CRC Press

96

Continuum Mechanics and Plasticity

in which AP is a principal direction of U. Note that this method of ﬁnding the deformed shape of an element is valid only when F is not a function of position. If F is a function of position, then the line elements must be divided into small increments, and this method is applied to each increment. Alternatively, the set of transformation equations (3.8) may be used to ﬁnd the deformed shape of the element point by point. The rotation of A B C D into A B C D is obtained by applying R to the deformed line element A B , A P , etc. given by (s1 to s4). The resulting line elements are √ 3 2 A B = − 1 2 0 √ 3 2 A P = 1 − 2 0 √ 3 2 A C = 1 − 2 0 √ 3 2 A D = 1 − 2 0

1 2 √ 3 2 0 1 2 √ 3 2 0 1 2 √ 3 2 0 1 2 √ 3 2 0

1 √ 0 2 3 2 3 √ 5 3 = 1 0 6 0 0 1 0 √ 3 √1 = 1 3 0 0 0 1

(s5)

(s6)

√ 1+ 3 √ 0 3+2 3 2 √ 3 3 + 5 3 = 1 0 6 0 1 0 √ 3 0 1 2 0 = 1 0 0 2 0 1

(s7)

(s8)

The two stages of deformation and rotation are shown in Figure 3.6. (c) Using (4.43), the square ABCD is ﬁrst rotated into A B C D by R. √ 3 2 1 − 2 0

1 2 √ 3 2 0

0 0 1 0 0 1

© 2005 by Chapman & Hall/CRC Press

1 √ 3 1 0

1 1 1 2 √ = 1 0 3 2 0 0 0

1 1 √ 3 0

√ 1+ 3 2 √ −1 + 3 2 0

√ 3 2 1 − 2 0

(t1)

Motion and Deformation

97

Note that the ﬁrst matrix is R, the second matrix is formed by the column vectors AB, AP, AC, and AD, and the third matrix is a collection of column vectors A B , A P , A C , and A D . In the second step, the square A B C D is deformed into A B C D by V, given by the following equation √ 1 1+ 3 1 0 1 2 2 √2 √ √ 3 3 −1 + 3 1 0 √ 2 2 2 3 0 1 0 0 0 √ √ 3+2 3 2 3 √ 1 3 3 3 = 1 1 1 0 0 0 0 0

5 2√3 1 2 0

√ 3 2 1 − 2 0

(t2)

In equation (t2), the ﬁrst matrix is V, the second matrix consists of column vectors A B , A P , A C , and A D , and the third matrix is a collection of column vectors A B , A P , A C , and A D . The two stages of rotation and deformation are shown in Figure 3.7. Comparing (s5 to s8) with (t2), we see that the results obtained from the left decomposition is the same as those from the right decomposition.

x2

n(1) v C

B

P⬙

B⬙

C⬙

B⬘

C⬘

R 30° A

D

D⬘ FIGURE 3.7 Left polar decomposition.

© 2005 by Chapman & Hall/CRC Press

x1

98

Continuum Mechanics and Plasticity

(d) A straight line passing through the origin is given by X2 = X1 tan θ

(u)

where θ is the angle between the line and the X1 axis. Substituting (a) into (u), this line is deformed into 1 + k x2 (v) x1 = tan θ The diagonal of the initial square element has θ = 45◦ . This angle is deformed into α where tan α =

1 x2 = x1 1+k

(w)

(e) A circle in the initial element is given by X12 + X22 = a2

(x)

where a is the radius. Substituting (a) into (x), this circle is deformed into x12 − 2kx1 x2 + (1 + k 2 )x22 = a2

(y)

It is observed that a circle is deformed into an ellipse with the semimajor axis making an angle of β with√the positive x1 axis. It can be shown that tan 2β = 2/k. Thus, when k = 2/ 3, β = 30◦ .

3.6

The Right Cauchy–Green Deformation Tensor

We now discuss some popular strain measures. Any strain measure is as good as the other as long as its deﬁnition is clear and correctly used. It is a matter of convenience to choose one measure over another for the description of the problem at hand. We discuss in this section a popular strain measure called the right Cauchy–Green tensor. Other popular measures are discussed in sections 3.9 and 3.10.

3.6.1

The Physical Meaning

Consider a line element dXR with length dS deforming into dxi with length ds. We have dxi =

© 2005 by Chapman & Hall/CRC Press

∂xi dXR ∂XR

(3.44)

Motion and Deformation

99

Dividing both sides of (3.44) by (ds dS), we obtain λni =

∂xi NR ∂XR

dXR dS

and ni =

(3.45)

where NR =

dxi ds

(3.46)

specify the directions (unit vectors) of the line element before and after deformation, respectively. The extension ratio (or stretch ratio) λ is deﬁned by λ=

ds dS

(3.47)

The notation λ is a popular notation for stretch ratio and should not be confused with the eigenvalues used in Chapter 2. Because of many notations, symbols, and quantities, the same notation may be used to mean different quantities. You should pay special attention to the deﬁnition of each notation used. Using (3.45), we form λ2 = (λni )(λni ) =

∂xi ∂xi NR NS = CRS NR NS ∂XR ∂XS

(3.48)

or λ2 = CRS NR NS

(3.49)

Note that CRS is a symmetric tensor and is positive deﬁnite. Given a deformation (3.8), F and C may be found. If we specify the initial direction NR of a line element, then the direction and magnitude of the deformed line element may be found using (3.45) and (3.49), respectively. In order to visualize the meaning of the diagonal terms C11 , C22 , C33 and the (1) off diagonal terms C12 , C23 , etc., of CRS , let us consider two line elements dXR (2) (1) (2) and dXR , which deform into dxi and dxi , respectively. The angle between the two line elements is in the initial conﬁguration and φ in the current conﬁguration as shown in Figure 3.8. The initial and deformed line elements are related by (1)

dxi

(2)

dxi

© 2005 by Chapman & Hall/CRC Press

∂xi (1) dXR ∂XR ∂xi (2) = dXR ∂XR =

(3.50) (3.51)

100

Continuum Mechanics and Plasticity

Then, we form the inner product of the two line elements (1)

(2)

dxi dxi

=

∂xi ∂xi (1) (2) (1) (2) dXR dXS = CRS dXR dXS ∂XR ∂XS

(3.52)

On the other hand, the inner product may be expressed in terms of the lengths of the line elements and the angle φ as (1)

(2)

dxi dxi

= ds1 ds2 cos φ12

(3.53)

where ds1 and ds2 are the lengths of the two line elements after deformation and φ12 is the inclusion angle. Let dS1 and dS2 be the lengths of the two line elements before deformation, then (1)

dXR (1) = NR dS1

(2)

dXR (2) = NR dS2

(3.54)

Using (3.54) and equating (3.52) to (3.53), we obtain ds1 ds2 (1) (2) cos φ12 = CRS NR NS dS1 dS2

(3.55)

From (3.55), we obtain information for C11 , C22 , C33 . Let us consider a line (1) (1) (1) element oriented initially along X1 , then N1 = 1, N2 = 0, N3 = 0. In this case, (3.55) reduces to

ds1 dS1

2

(2)

= C11 = λ1

(3.56a)

We note that C11 is related to the extension ratio λ1 along X1 . Similarly, if we consider line elements oriented initially along X2 and X3 , respectively, we obtain C22 =

ds2 dS2

2

and C33 =

ds3 dS3

2 (3.56b,c)

We now consider the angle changes between the two line elements as shown in Figure 3.8. In a special case, the two line elements are initially 90◦ (2) (1) to each other. Let dXi be along the X1 direction and dXi be along the (1) (2) X2 direction, then the unit normals are NR ∼ [1, 0, 0] and NS ∼ [0, 1, 0]. Equation (3.55) now reduces to ds1 ds2 cos φ12 = C12 dS1 dS2

© 2005 by Chapman & Hall/CRC Press

(3.57)

101

i

dx (1

)

Motion and Deformation

(1)

dX R

(2)

dx i

Φ

dX

(2 R )

FIGURE 3.8 Deformation of two line elements.

Making use of (3.56), (3.57) becomes cos φ12 = √

C12 √

C11 C22

(3.58)

Note that (3.58) relates C12 to φ12 , which is the angle after deformation. The angle φ12 may no longer be 90◦ and the two line elements are in general not oriented along the coordinate axes after deformation. Using a similar procedure, we relate C23 to φ23 and C31 to φ31 . These equations are summarized and we write cos φRS = √

CRS √ CRR CSS

(R, S not summed)

(3.59)

It may be concluded that the diagonal terms C11 , C22 , C33 are related to the extension ratios λ1 , λ2 , λ3 , respectively; they represent the stretching along the coordinate directions; the off-diagonal terms C12 , C23 , C31 are related to the current angles φRS , respectively; they are different from the initial angles RS and, therefore, represent shearing deformation. Finally, we remark that, if the triad formed by the three initial line elements are along the principal directions of CRS , then C12 = C23 = C31 = 0. From (3.59), we ﬁnd φ12 = φ23 = φ31 = 90◦ , that is, the triad remains mutually perpendicular to each other after deformation. Furthermore, in the undeformed state, CRS does not vanish, that is, C11 = 1, C22 = 1, C33 = 1, and C12 = cos φ12 = 0, etc., or we may write CRS = δRS in the undeformed conﬁguration.

3.6.2

Transformation Properties of CRS

In this subsection, we consider the transformation properties of CRS with respect to the rotation and translation of either the material coordinate system ¯ R be an alternative material system, or the spatial coordinate system. Let X

© 2005 by Chapman & Hall/CRC Press

102

Continuum Mechanics and Plasticity

which is related to XR by ¯ R = MSR XS + aR X

(3.60)

where MRS is a rotation matrix, that is, MTR MTS = δRS = MRT MST

with |MRS | = 1

(3.61)

Both M and a are independent of XR . Also, let x¯ i be an alternative spatial system such that x¯ i = Qji (t)xj + bi (t)

(3.62)

where Qij Qik = δjk = Qji Qki

with |Qij | = 1

(3.63)

¯ R and x¯ i differs from the original system by a rigid-body Note that each of X rotation plus a translation. 3.6.2.1 Rotation and translation of material system ¯ R , the expressions of CRS are, respectively, Referring to XR and X CRS =

∂xi ∂xi ∂XR ∂XS

and

∂xi ∂xi C¯ RS = ¯ R ∂X ¯R ∂X

(3.64)

By the chain rule of differentiation, we have CRS =

¯ T ∂xi ∂ X ¯V ∂xi ∂xi ∂ X ∂xi = MRT M = MRT MSV C¯ TV ¯ ¯ ¯ ¯ V SV ∂ XT ∂XR ∂ XV ∂XS ∂ XT ∂X

(3.65)

or C¯ RS = MTR MVS CTV

(3.66)

Therefore, CRS transforms as a second-order tensor with rotation of the material system but it remains invariant with translation of the material system. This result is expected because both subscripts of CRS refer to the material system. We note that C¯ RS in this subsection should not be confused with the C¯ RS matrix referring to the principal coordinate system and used in most other sections.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

103

3.6.2.2 Rotation and translation of the spatial system Referring to xi and x¯ i , the expressions of CRS are, respectively, CRS =

∂xi ∂xi ∂XR ∂XS

and CRS =

∂ x¯ i ∂ x¯ i ∂XR ∂XR

(3.67)

The second equation in (3.67), by use of (3.62), is further written as CRS =

∂xj ∂ x¯ i ∂xj ∂ x¯ i ∂xk ∂xk = Qji Qki ∂xj ∂XR ∂xk ∂XS ∂XR ∂XS

= δjk

∂xj ∂xk ∂xk ∂xk = = CRS ∂XR ∂XS ∂XR ∂XS

(3.68)

We conclude that CRS remains invariant with rotation and translation of the spatial system. This is also expected, because both subscripts of CRS refer to the material system and it does not matter which spatial coordinate system we use.

3.6.3

Eigenvalues and Eigenvectors of CRS

CRS is a symmetric matrix and it has three real eigenvalues and three real eigenvectors. The properties of eigenvalues and eigenvectors are discussed ¯ R to denote the principal coordinate system of CRS . in Section 2.7. We use X The principal values (eigenvalues) C¯ RS are related to CRS by

C¯ RS = QPR QQS CPQ

ds1 dS1 = 0 0

2

0 ds2 dS2 0

2

2 λ1 =0 0 0 ds3 2 0

0

0

λ22

0

0

λ23

dS3 (3.69)

We see that, when CRS are expressed in the principal frame, it becomes a (R) diagonal matrix. The eigenvectors, or the principal directions, are nC with R = 1, 2, and 3. Figure 3.9 shows the eigenvectors in the neighborhood N0 of an undeformed body. Whatever the deformation of N0 , there exists one set of three line elements, which are mutually orthogonal. The three line elements may extend during deformation and the triad may rotate, but the angles between them will always be right angles.

© 2005 by Chapman & Hall/CRC Press

104

Continuum Mechanics and Plasticity

nC(3) N0

nC(2) nC(1)

R0 3 2 1

FIGURE 3.9 Eigenvectors in the neighborhood N0 .

3.6.4

Principal Invariants of CRS

Similar to the stress invariants discussed in Section 2.12, we deﬁne the invariants for CRS as (3.70) I1 = CRR = C11 + C22 + C33 I2 = tr(cof. C) = I3 tr(C−1 )

(3.71)

I3 = det C

(3.72)

We now discuss the geometric signiﬁcance of I1 , I2 , and I3 . In principal axes, the invariants I1 , I2 , and I3 may be associated with the geometric properties of a material element. The matrix of C is a diagonal matrix as shown in (3.69). In this system, the expressions for the invariants are I1 = λ21 + λ22 + λ23

(3.73)

I2 = λ22 λ23 + λ21 λ23 + λ21 λ22 1 1 1 1 1 1 = λ21 λ22 λ23 + 2 + 2 = I3 + 2 + 2 = I3 tr(C−1 ) λ21 λ2 λ3 λ21 λ2 λ3 I3 = λ21 λ22 λ23

(3.74) (3.75)

In the case that the initial lengths are dS1 = 1, dS2 = 1, and dS3 = 1, (3.69) reduces to

ds21 C= 0 0

© 2005 by Chapman & Hall/CRC Press

0 ds22 0

0 0 ds22

(3.76)

Motion and Deformation

105

ds3

3

P 2

O

ds 1

d s2

1 FIGURE 3.10 Deformed cuboid for geometric interpretations of strain invariants.

and I1 = |OP|2 = ds21 + ds22 + ds23

(3.77)

I2 = sum of squares of areas of three mutually perpendicular faces of deformed cuboid 2 ds 0 ds21 0 ds21 2 = + + 0 ds2 0 ds2 0 3

3

0 = ds22 ds23 + ds21 ds23 + ds21 ds22 ds2 2

(3.78) I3 = square of volumes of deformed unit cuboid = (ds1 ds2 ds3 )

2

(3.79)

The above geometric interpretations are clear when we refer to Figure 3.10.

3.7

Deformation of Volume and Area of a Material Element

We investigate ﬁrst the deformation of a volumetric element within the neighborhood N0 and then investigate how an area element deforms during deformation. The initial volume of an inﬁnitesimal parallelepiped within N0 is dV0 , which is the scalar triple product of the three vectors

© 2005 by Chapman & Hall/CRC Press

106

Continuum Mechanics and Plasticity

forming the sides of the parallelepiped. The deformed volume is denoted by dV. We have (1) (2) (3) dV0 = dX(1) · dX(2) × dX(3) = ePQR dXP dXQ dXR

(3.80)

∂xi (1) ∂xj (2) ∂xk (3) dXP dXQ dXR ∂XP ∂XQ ∂XR ∂xi ∂xi ∂xj ∂xk (1) (2) (3) dX (1) dX (2) dX (3) = eijk dXP dXQ dXR = ePQR Q R ∂XP ∂XQ ∂XR ∂XP P (3.81) (1)

(2)

(3)

dV = eijk dxi dxj dxk = eijk

From (3.80) and (3.81), we obtain ∂xi dV = ∂X

P

dV0

or

∂xi dV = det F = dV0 ∂XP

(3.82)

Let dm be the mass of the volumes dV and dV0 and ρ and ρ0 be the densities of dV and dV0 , respectively. Equation (3.82) may be rewritten as ∂xi ρ0 = det F = J = ρ ∂XP

(3.83)

∂xi ∂xi = |FT · F| = |FT | |F| = |F|2 I3 = |CRS | = ∂XR ∂XS

(3.84)

Now that

we ﬁnd from (3.83) and (3.84) that I3 =

dV dV0

2

=

ρ0 ρ

2 (3.85)

We consider next the deformation of an area element. Referring to Figure 3.11, (2) (1) line elements dXR and dXR form the initial area dA, which has a unit (1) (2) normal of NR . The two line elements deform into dxi and dxi , and area dA deforms into da with unit normal ni . The two areas can be expressed as vectors given by dAR = NR dA

© 2005 by Chapman & Hall/CRC Press

and

dai = ni da

(3.86)

Motion and Deformation dA R N =

M⬙

R dA

d

) (2 XR

d

M

107

=n

id

a

ai

dA

m⬙ ) (2 dx i

dX (1) R

da

m dx (1) i

M⬘

m⬘ (After Deformation)

(Before Deformation) FIGURE 3.11 Deformation of area element.

In addition, the undeformed area is (1)

(2)

with (dA)2 = dAR dAR

(3.87)

(1)

(2)

with (da)2 = dai dai

(3.88)

dAR = eRST dXS dXT and the deformed area is dai = eijk dxj dxk

We now proceed to ﬁnd the relation between the two areas. By way of the chain rule of differentiation, (3.87) can be written as dAR = eRST

∂XS ∂XT (1) (2) dx dxn ∂xm ∂xn m

(3.89)

Multiplying (3.89) by ∂XR /∂xk , we obtain ∂XS ∂XT ∂XR (1) (2) ∂XM ∂XR (1) dAR = eRST dxm dxn = dxn(2) ekmn dxm ∂xk ∂xm ∂xn ∂xk ∂xr ∂XM dak = (3.90) ∂x r

Equation (3.88) and the identity discussed in Example 2.7 have been used in the above derivation. Thus, we may conclude that ∂XM ∂XR dak dAR = ∂xk ∂xr

(3.91)

or using (3.83), dai = J

∂XR dAR ∂xi

or

da = J(F−1 )T · dA

Equation (3.92) relating dAR to dai is called Nanson’s formula.

© 2005 by Chapman & Hall/CRC Press

(3.92)

108

3.8

Continuum Mechanics and Plasticity

The Left Cauchy–Green Deformation Tensor

The left Cauchy–Green tensor B is deﬁned in (3.41). It is seen that both subscripts of Bij refer to the spatial coordinate system. B is invariant with rotation of the material system and transforms as a second-rank tensor with rotation of the spatial system. We now show that the invariants of B, denoted by IB , II B , and III B , coincide with those of C, denoted by IC = I1 , II C = I2 , and III C = I3 . From (3.70), we have ∂xi ∂xi = Bii = IB ∂XR ∂XR

IC = CRR =

(3.93)

and from (2.79), the second invariant is II B =

1 2

IB2 − tr B2

(3.94)

where B2 = Bip Bpj and the trace of this expression is ∂xi ∂xp ∂xp ∂xi tr B = Bip Bpi = = ∂XR ∂XR ∂XS ∂XS 2

∂xi ∂xi ∂XR ∂XS

= CRS CRS = tr C2

∂xp ∂xp ∂XR ∂XS

(3.95)

Substituting (3.93) and (3.95) into (3.94), we obtain II B = II C

(3.96)

For the third invariant, we have from (3.72) and (3.84) III C = |C| = |FT · F| = |FT ||F| = |F|2

(3.97)

III B = |F · FT | = |F||FT | = |F|2

(3.98)

On the other hand,

Comparing (3.97) and (3.98), we ﬁnd III B = III C

3.9 3.9.1

(3.99)

The Lagrangian and Eulerian Strain Tensors Deﬁnitions

The two classical strain measures discussed in this section are widely used in mechanics literature. Usually, they are derived from a different approach

© 2005 by Chapman & Hall/CRC Press

109

P

dX

u

dx

Motion and Deformation

p Nt

X

N0

x

3 2 1 FIGURE 3.12 The displacement vector.

than the one given here. Having discussed the right and left Cauchy–Green deformation tensors, we may deﬁne the Lagrangian and Eulerian strains as 2E = C − 1

(3.100)

2e = 1 − B−1

(3.101)

where E is the Lagrangian strain tensor (also known as Green’s tensor) and e is the Eulerian strain tensor. We point out, from (3.100), that C is positive for E > − 12 . In this discussion, we observe that deformation of a continuum may be described by different strain measures. In fact, there are several alternative measures of deformation that are being used in the literature. The displacement vector u introduced in (3.3) is now considered. Refer to Figure 3.12 and let the material and spatial coordinate systems coincide for simplicity. If a material point P moves to p during deformation, the vector from P to p is the displacement vector u. We may write x =X+u

or

xi = δiR XR + ui

(3.102)

Using (3.102), (3.100) becomes ∂xm ∂xm − δRS ∂XR ∂XS ∂ (δmM XM + um ) ∂ (δmN XN + um ) = − δRS ∂XR ∂XS ∂um ∂um δmS + − δRS = δmR + ∂XR ∂XS

2ERS = CRS − δRS =

= δmR δmS + δmR

© 2005 by Chapman & Hall/CRC Press

∂um ∂um ∂um ∂um + δmS + − δRS ∂XS ∂XR ∂XR ∂XS

(3.103)

110

Continuum Mechanics and Plasticity

Note that we choose to have the origin of the material and spatial coordinate systems coincide. In general, they may not coincide, but since the vector connecting the two origins is a constant, it drops out in the differentiation. Thus, (3.103) may be simpliﬁed to yield ERS

1 = 2

∂uS ∂uR ∂uk ∂uk + + ∂XS ∂XR ∂XR ∂XS

(3.104)

Equation (3.104) is known as the strain–displacement relation. Similarly, from (3.101), we obtain 1 eij = 2

∂uj ∂uR ∂uR ∂ui + − ∂xj ∂xi ∂xi ∂xj

(3.105)

where uR and ui are respectively components of the displacement vector u in the material and spatial coordinate systems. Since both coordinate systems are Cartesian and coincide in this consideration, uR is the same as ui . Also, XR is the same as Xi . Some remarks are in order. 1. Both ERS and eij are symmetric tensors. 2. A line element dXR with length dS in the neighborhood of N0 deforms into dxi with length ds in the neighborhood of Nt . It is possible to show that ds2 − dS2 = 2ERS dXR dXS = 2eij dxi dxj

(3.106)

3. For small deformation, that is, ∂ui /∂XR 1, and ∂uR /∂xj 1, but ui may not be small, we can approximately write 1 Eij ∼ = 2

∂uj ∂ui + ∂Xj ∂Xi

1 ∼ = eij ∼ = 2

∂uj ∂ui + ∂xj ∂xi

= εij

(3.107)

It is not necessary to distinguish the material coordinates XR from the spatial coordinates xi (see Example 3.4). The tensor εij is called the inﬁnitesimal strain tensor or the engineering strain. Both E and e reduce to ε when an approximation is made such that the second and the higher powers of the displacement gradients are neglected. 4. On the other hand, the inﬁnitesimal strain tensor may be mathematically deﬁned by 1 εij = 2

© 2005 by Chapman & Hall/CRC Press

∂uj ∂ui + ∂xj ∂xi

(3.108)

Motion and Deformation

111

Physically, ε cannot be an exact measure of deformation, because it does not remain constant in a rigid-body rotation. In a counterclockwise rigid-body rotation through an angle α about the positive X3 axis, the transformation of the position vector of a material point is given by (see Example 1.6) x1 = X1 cos α − X2 sin α,

x2 = X1 sin α + X2 cos α,

x3 = X3 (3.109)

and the displacement components are u1 = −X1 (1 − cos α) − X2 sin α, u2 = X1 sin α − X2 (1 − cos α),

u3 = 0

(3.110)

Using (3.108), the inﬁnitesimal strain ε is determined to be

−(1 − cos α) 0 0 −(1 − cos α) εij = 0 0

0 0 0

(3.111)

It is seen that ε11 and ε22 are not 0. However, if α is small, then these quantities are small and may be neglected. Although the inﬁnitesimal strain tensor is not an exact measure of deformation, it is convenient for use in the applications involving small strains. An advantage of this strain tensor is its linear relation with respect to the displacement gradient. This allows for the application of the techniques of linear analysis in solving boundary-value problems in the linear theory of elasticity, and also helps keep the equations of the theory of plasticity simple. Nevertheless, in using (3.108), we must keep in mind that the rigid-body rotation has to be small. Show that, in the case of small displacement gradient, we may write ∂ui /∂xj ∼ = ∂ui /∂Xj and it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi .

EXAMPLE 3.4

Solution From (3.102), we have xi = Xi + ui

(a)

∂ui ∂Xi = δij − ∂xj ∂xj

(b)

By differentiating (a), we obtain

© 2005 by Chapman & Hall/CRC Press

112

Continuum Mechanics and Plasticity

In the symbolic notation, (b) can be written as ∂u = 1 − F−1 = 1 − {1 + (F − 1)}−1 ∂x = 1 − {1 − (F − 1) + (F − 1)2 − (F − 1)3 + · · · } = (F − 1) − (F − 1)2 + (F − 1)3 − · · ·

(c)

in which the binomial expansion was used. In the index notation, the factor (F − 1) is ∂xi ∂ui − δij = ∂Xj ∂Xj

(d)

∂ui ∂ui ∂ui ∂uR ∂ui ∂uR ∂uS = − + − ··· ∂xj ∂Xj ∂XR ∂Xj ∂XR ∂XS ∂Xj

(e)

By substitution, (c) becomes

Hence, by neglecting the higher-order terms in the displacement gradient, we may write ∂ui ∼ ∂ui = ∂xj ∂Xj

(f)

and it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi . 3.9.2

Geometric Interpretation of the Strain Components

We consider here as in Section 3.6.1 a line element dXR with length dS deforming into dxi with length ds. We relate the stretching of this line element to the components of E rather than to the components of C. From the usual deﬁnition of strain, we deﬁne the relative elongation of the line element as ε=

ds − dS ds = −1=λ−1 dS dS

(3.112)

This deﬁnition of relative elongation is valid for large deformation as well. From (3.106), we have ds2 = dS2 + 2ERS dXR dXS

(3.113)

Dividing (3.113) by dS2 , we obtain λ2 =

dXR dXS ds2 = 1 + 2ERS = 1 + 2ERS NR NS dS dS dS2

© 2005 by Chapman & Hall/CRC Press

(3.114)

Motion and Deformation

113

or λ = [1 + 2ERS NR NS ]1/2

(3.115)

where NR denotes the initial direction of the line element. We have discarded the “−” solution in (3.115), since λ = ds/dS ≥ 0 always. Therefore, the relative elongation is from (3.112) given by ε = λ − 1 = [1 + 2ERS NR NS ]1/2 − 1

(3.116)

If we know ERS and specify a direction NR , then from (3.116) we obtain the elongation of this line element. Equation (3.115) may be compared with (3.49), in which the components of C are used. These expressions show that the extension ratio can be obtained by the use of two different strain measures. The two equations are related by λ2 = 1 + 2ERS NR NS = NR NR + 2ERS NR NS = (δRS + 2ERS )NR NS = CRS NR NS

(3.117)

We now consider the meaning of the diagonal and off-diagonal components of the ERS matrix. To discuss the diagonal component E11 , let us consider a line element in the X1 direction before deformation. We then have N1 = 1, N2 = 0, and N3 = 0; and, from (3.114), we obtain λ211 = 1 + 2E11

and ε11 = λ11 − 1 =

1 + 2E11 − 1

(3.118)

Equation (3.118) shows that E11 is related to the stretching of the line element, which is initially in the X1 direction. Similarly, if we consider line elements initially along X2 and X3 directions, respectively, we get ε22 =

1 + 2E22 − 1

and ε33 =

1 + 2E33 − 1

(3.119)

Starting with the Eulerian strain components eij , we can also obtain expressions for the relative elongations for ﬁbers, which after deformation are in the directions of the x1 , x2 , and x3 axes. However, the interpretation of e11 , e22 , and e33 as the relative elongations of ﬁbers can only be justiﬁed for small strain. If we choose a line element, which is in the x1 direction after deformation, then (3.106) leads to (ds − dS)(ds + dS) = 2eij dxi dxj = 2e11 n1 n1 ds2 = 2e11 ds2

(3.120)

By use of the deﬁnition of relative elongation, (3.120) may be written as ds − dS ds 2ds = e11 ≈ e11 dS dS ds + dS © 2005 by Chapman & Hall/CRC Press

(3.121)

114

Continuum Mechanics and Plasticity

The last expression of (3.121) is true only for small deformation that ds ≈ dS. In this case, e11 may be interpreted as the relative elongation for ﬁbers in the x1 direction, and we note that for small deformation x1 ≈ X1 . However, in large deformation, no simple correlation between e11 and relative elongation can be found from (3.121). To investigate the off-diagonal terms of ERS , let us consider two line (1) (2) (1) (2) elements dXR and dXR , which deform into dxi and dxi , respectively. The angle between the two line elements is in the initial conﬁguration and (1) φ in the current conﬁguration as shown in Figure 3.8. The dot product of dXR (2) and dXR is (1)

(2)

dS1 dS2 cos = dXR dXR (1)

and the dot product of dxi

(2)

and dxi

(3.122)

is (1)

(2)

ds1 ds2 cos φ = dxi dxi

(3.123)

Subtracting (3.122) from (3.123), we obtain (1)

(2)

(1)

(2)

ds1 ds2 cos φ − dS1 dS2 cos = dxi dxi − dXR dXR ∂xi ∂xi (1) (2) = − δRS dXR dXS ∂XR ∂XS ∂ui ∂ui (1) (2) = + δiR + δiS − δRS dXR dXS ∂XR ∂XS (1)

(2)

= 2ERS dXR dXS

(3.124)

The relations in (3.103) are used in the derivation of (3.124). Dividing the above expression by dS1 dS2 , we obtain (1)

(2)

dXR dXS ds1 ds2 (1) (2) cos φ − cos = 2ERS = 2ERS NR NS dS1 dS2 dS1 dS2

(3.125)

This relation may be further simpliﬁed by use of (3.112), which, for the two line elements, are ds1 = λ1 dS1

and

ds2 = λ2 dS2

(3.126)

Using (3.126), (3.125) may be solved to yield (1)

cos φ =

© 2005 by Chapman & Hall/CRC Press

(2)

2ERS NR NS + cos λ1 λ 2

(3.127)

Motion and Deformation

115

where is the angle between the two line elements before deformation (1) (2) and φ is the angle after deformation. Given , ERS , NR , and NS , the deformed angle φ may be determined. Note that the stretch ratios λ1 and λ2 are determined from (3.115). To investigate the meaning of E12 , E23 , E31 , let us consider some special cases. If = 90◦ , that is, the two line elements are perpendicular to each other before deformation, then cos = 0. In addition, let cos φ = cos(90◦ − θ ) = sin θ, where θ is the angle change due to deformation, then (3.127) reduces to (1)

sin θ =

(2)

2ERS NR NS λ 1 λ2

(3.128)

Since θ is generally not 0 from (3.128), we may conclude that two initially perpendicular line elements (not along the coordinate axes) do not remain perpendicular after deformation. If the two line elements are respectively (1) (1) (1) lying along the X1 and X2 axes initially, then N1 = 1, N2 = N3 = 0 and (2) (2) (2) N2 = 1, N1 = N3 = 0, and from (3.128) E12 is related to θ12 . Similarly, we ﬁnd the expressions for other off-diagonal terms of ERS (R = S). The relations are summarized as sin θ12 =

2E12 , λ1 λ 2

sin θ23 =

2E23 , λ 2 λ3

sin θ13 =

2E13 λ 1 λ3

(3.129)

We observe from (3.129) that the off-diagonal terms of ERS are related to the shearing deformations and that an initially orthogonal triad with elements along the XR directions will no longer be orthogonal after deformation. We consider a special case, where X1 , X2 , and X3 are principal directions. Then, E12 = E23 = E31 = 0 and E11 = E1 , E22 = E2 , E33 = E3 . If the two line elements are respectively lying along X1 and X2 initially, then from (3.129) we obtain θ12 = 0, which means that there is no angle change, that is, φ = = 90◦ . Similarly, we show that θ23 = θ31 = 0. This ﬁnding has the implication that a rectangular triad having elements in the three principal directions before deformation remains rectangular (does not have angle changes) after deformation. The volume element formed by the triad is rotated and may be stretched. However, if, before deformation, the triad is in directions other than the principal directions, then there are angle changes after deformation even if ERS refers to the principal directions. The angle changes for this case are calculated from (3.128).

3.9.3

The Volumetric Strain

Using (3.82) and (3.100), we have

dV dV0

© 2005 by Chapman & Hall/CRC Press

2

= |FT · F| = |C| = |δRS + 2ERS |

(3.130)

116

Continuum Mechanics and Plasticity

Since the above expression is the third invariant of C, a simpliﬁed expression is obtained by using the principal coordinate system. Thus,

dV dV0

2

= (1 + 2E1 ) + (1 + 2E2 )(1 + 2E3 ) = 1 + 2(E1 + E2 + E3 ) + 4(E1 E2 + E1 E3 + E2 E3 ) + 8E1 E2 E3 (3.131)

or

dV dV0

2

= 1 + 2IE + 4II E + 8III E

(3.132)

where IE , II E , and III E are the principal invariants of E. But, from (3.116), we note that 1 + ε1 =

1 + 2E1

(3.133)

in which ε1 is the relative elongation along principal direction 1. Using (3.133), (3.131) becomes dV = (1 + ε1 )(1 + ε2 )(1 + ε3 ) = λ1 λ2 λ3 dV0

(3.134)

We note that the volumetric strain for small deformation is dV − dV0 dV = − 1 = (1 + ε1 )(1 + ε2 )(1 + ε3 ) − 1 ≈ ε1 + ε2 + ε3 (3.135) dV0 dV0 by neglecting the high-power terms in ε1 , ε2 , or ε3 . In the ﬁnite deformation, the volumetric strain can be deﬁned by (dV − dV0 )/dV, which leads to the logarithmic volumetric strain of ln(dV). EXAMPLE 3.5

Consider the deformation governed by x 1 = α1 X 1 ,

x2 = α2 X2 ,

x3 = α3 X3

(a)

where αi are constants. In a one-dimensional stretching along the 1 direction, determine the values of E11 , e11 , the relative elongation ε, and the true strain εlog , if α1 takes the values of 1.01, 1.02, 1.05, 1.10, and 1.20. Compare these values with the engineering strain ε eng .

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

117

Solution Using (a), we ﬁnd

α12 T [C] = [F] [F] = 0 0

0 α22 0

0 0 α32

and [B]−1

1 α2 1 = 0 0

0 1 α22 0

0

0 1

(b)

α32

Substituting (b) into (3.100) and (3.101), we obtain (C11 − 1) = 12 (α12 − 1) 1 1 1 −1 1− 2 = (1 − B11 ) = 2 2 α1

E11 = e11

1 2

(c) (d)

Since N1 = 1, N2 = N3 = 0, the relative elongation ε may be found from (3.116) and (c) as ε = α1 − 1

(e)

Note that this result is the same as that obtained from the deﬁnition of engineering strain, where ε eng =

x−X = α1 − 1 X

(f)

The true strain is deﬁned by dε log = dx/x. If the initial strain is 0 and the initial length of the specimen is X, this expression may be integrated to ﬁnd ε log = ln

x X

= ln α1

(g)

Expressions (c) to (g) are plotted in Figure 3.13 against α1 . The curve for the engineering strain εeng is a straight line. The curve for E11 lies above the straight line and the curves for εlog and e11 lie below the straight line. We note that, at a strain of εeng = 0.05, the corresponding logarithmic strain is εlog = 0.0488, which is 2.4% smaller than ε eng ; at εeng = 0.1, ε log = 0.0953, which is 4.9% smaller than εeng ; and at εeng = 0.2, ε log = 0.1823, which is 9.7% smaller than εeng .

© 2005 by Chapman & Hall/CRC Press

118

Continuum Mechanics and Plasticity E11 e11

0.2

eng log

Strain

0.15 0.1 0.05 0 1.0

1.15

1.1 1

1.05

1.2

FIGURE 3.13 Comparison of strain measures in one-dimensional stretching.

3.10

Other Strain Measures

Several other strain measures have been used in the literature. We mention in this section two families of strains, which are deﬁned based on the stretch tensors U and V discussed in Section 3.5. Both U and V are positive, symmetric tensors, they share the same eigenvalues λi and their eigenvectors are related by the transformation given by equation (r) of Example 3.3. In the proposed strain measures, the eigenvalues are a function of λi such that εi = f (λi )

(3.136)

A useful form for function f is given by λκi − 1 , κ = ln λi ,

f (λi ) =

κ = 0

(3.137)

κ=0 (i)

(i)

The two families of strains are written using either nu or nv as their eigenvectors. Thus, E = f(U) =

f (λi )nu(i) ⊗ nu(i)

i

or

e = f(V) =

f (λi )nv(i) ⊗ nv(i)

i

(3.138) where E may be called the generalized Lagrangian strain and e the generalized Eulerian strain. Some commonly used strain measures may be

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

119

obtained from (3.138). They are Engineering strain (κ = 1): ε eng = λ − 1 Logarithmic strain (κ = 0):

ε log = ln λ

Lagrangian strain (κ = 2):

E = 12 (λ2 − 1) 1 1 e= 1− 2 2 λ

Eulerian strain (κ = −2):

(3.139)

The last two strain measures are written in the spectral form as E=

1 i

2

(λ

2

− 1)nu(i)

⊗ nu(i)

and e =

1 1 − 2 nv(i) ⊗ nv(i) 2 λ

1 i

(3.140)

A disadvantage of strain measures deﬁned by (3.138) is the necessity of calculating the principal components ﬁrst and then performing axes transformation to the actual axes. A popular method to avoid axes transformation is to use strain measures with κ = 2 or −2 so that the strain tensors may be directly calculated from either the stretch tensors U and V or the right and left Cauchy–Green tensors C and B.

3.11

Material Rate of Change

We discussed the concept of deformation and its measures in the earlier sections. As mentioned earlier, the deformation describes the geometrical change of a material element between the current and the reference conﬁgurations corresponding to two different ﬁxed times. The study now extends to the motion of the body, which is a family of deformations continuously varying in time. The material rate of change (or material derivative) is an important concept used in the description of the motion and we discuss it in this section. The material rate of change of a physical quantity φ is the rate of change of φ with respect to a particle. This rate is also known as the substantial derivative in ﬂuid mechanics. There are material and spatial descriptions for the material rate of change and we discuss them in this section.

3.11.1

Material Description of the Material Derivative

In the material description, X is held constant, and the material derivative is the same as the partial derivative with respect to time t. Therefore, we write D ∂φ(X, t) φ(X, t) = Dt ∂t

© 2005 by Chapman & Hall/CRC Press

(3.141)

120

Continuum Mechanics and Plasticity

or in the index notation D ∂φ(XR , t) φ(XR , t) = Dt ∂t 3.11.2

(3.142)

Spatial Description of the Material Derivative

In the spatial description, φ is a function of x and t. The material derivative of φ is the total derivative of φ, differentiating with respect to both variables. Thus, D ∂φ(x, t) ∂φ ∂x φ(x, t) = + · Dt ∂t ∂x t ∂t X

(3.143)

Note that the last differentiation is carried out by keeping X constant. This is so because we are considering the material derivative. The particle velocity has been discussed in (3.6), and using the expression, (3.143) becomes D ∂φ(x, t) −−−−→ φ(x, t) = + Grad φ · v(x, t) Dt ∂t

(3.144)

In the last expression of (3.144), notation v represents v(x, t). The same notation v may be used to represent v(X, t) in the material description. These are actually two different functions denoting the same velocity. But for the sake of simplicity in notations, we use the same notation v. The independent variables of the function should be speciﬁed in case confusion arises. In a similar manner, we discuss the material differentiation of a vector. Acceleration, which is the material derivative of the velocity vector, is a good example and is given by f=

Dv ∂v = + (Grad v) · v Dt ∂t

(3.145)

The last expression of (3.145) may be derived by writing Grad v ≡

∂vi ei ⊗ e j ∂xj

=∇ ⊗v

(3.146)

Thus, (Grad v) · v = =

© 2005 by Chapman & Hall/CRC Press

∂vi ∂vi ei ⊗ ej · vk ek = vk ei (ej · ek ) ∂xj ∂xj

∂vi ∂vi vk ei δjk = vk ei ∂xj ∂xk

(3.147)

Motion and Deformation

121

Using (3.147), the index form of (3.145) is fi =

∂vi ∂vi Dvi = + vk Dt ∂t ∂xk

(3.148)

Generally, the material derivative in the spatial description is represented by the following operator D ∂ ∂ = + vk Dt ∂t ∂xk

(3.149)

If this operator is applied to a function φ(x, t), then the ﬁrst term indicates the local rate of change, which is the contribution of the time dependence of φ. This term may also be called the transient term. The second term is the convective term, which is the contribution by the motion of the particle. To illustrate this point, let us consider ﬂuid ﬂowing in a tube and we assume that the ﬂow is steady and is one-dimensional along the x direction (see Figure 3.14). In a steady ﬂow, the velocity at any location x does not change with time. The observer sitting at a location x does not see any change of v, so that ∂v/∂t = 0. However, the velocity may differ from one location to the other. The acceleration of the particle is then given by Acceleration =

change of velocity (∂v/∂x)x (∂v/∂x)vt ∂v = = =v time increment t t ∂x (3.150)

This acceleration is known as the convective acceleration and is due to the motion of the ﬂuid. In a nonsteady ﬂow, the velocity changes with time at a ﬁxed station x. It changes from v to v + (∂v/∂t)t in time interval t and the acceleration at this station x is given by Acceleration =

change of velocity (∂v/∂t)t ∂v = = time increment t ∂t ∆x = v∆t

x t =t velocity v = v FIGURE 3.14 Fluid ﬂowing in a tube.

© 2005 by Chapman & Hall/CRC Press

x + ∆x t = t + ∆t ∆v velocity = v + ∆x ∆x

(3.151)

122

Continuum Mechanics and Plasticity

This is the transient term of acceleration and there is no convective acceleration because we consider the acceleration at a ﬁxed station. In the general case, that is, the station is not ﬁxed at x and the ﬂow is nonsteady, the total acceleration is therefore f=

∂v ∂v +v ∂t ∂x

(3.152)

In summary, the material rate of change, which is the rate of change of a physical quantity with respect to a speciﬁed particle, can be speciﬁed either by using a material description or a spatial description. In the material description, XR is speciﬁed and the particle is colored red. The material rate for a physical quantity is seen by an observer sitting on top of the particle and moving with the particle. Thus, the material rate changes with respect to t only. In the spatial description, the spatial coordinate changes (convects) with the particle, and the material rate of change has two parts, the convective and the transient. Thus, the acceleration of a speciﬁed (red) particle is what an observer who stands still in the laboratory sees.

3.12

Dual Vectors and Dual Tensors

The concept of dual vector and dual tensor is useful in the subsequent sections of this chapter. Given a tensor of the second-rank Tij , let us form the following vector ti = − 12 eijk Tjk

(3.153)

Vector ti is called the dual vector (or axial vector) of tensor Tij . We can show that the dual vector depends only on the antisymmetric part of tensor Tij . Thus, ti = − 12 eijk Tjk = − 12 eijk TjkS + TjkA = − 12 eijk TjkA

(3.154)

in which the superscripts S and A denote the symmetric and the antisymmetric parts, respectively. We note that the dual vector of a symmetric tensor vanishes and it has the components given below T − T32 1 23 T31 − T13 t=− 2 T −T 12

(3.155)

21

which forms a column vector. If we multiply both sides of (3.153) by eijk , we obtain eijk ti = − 12 eijk eirs Trs = − 12 (δjr δks − δjs δkr )Trs = − 12 (Tjk − Tkj )

© 2005 by Chapman & Hall/CRC Press

(3.156)

Motion and Deformation

123

Therefore, if Tij is symmetric, then from (3.156), ti = 0; and if Tij is antisymmetric, eijk ti = −Tjk , that is, Tjk = −eijk ti

(3.157)

Tjk is called the dual tensor of a given vector ti and the dual tensor is antisymmetric with components given by

0 T = t3 −t2

−t3 0 t1

t2 −t1 0

(3.158)

Use the dual vector–dual tensor concept to describe the angular velocity of rigid-body rotation of a continuum.

EXAMPLE 3.6

Solution Let us consider a rigid body that instantaneously rotates about an axis passing through point P in the body, and P has position vector r0 (see Figure 3.15). Note that for an inﬁnitesimal rotation, we consider the increments of angular and linear displacements dθ and dx, respectively, instead of angular and linear velocities ω = dθ/dt and v = dx/dt and similar results may be obtained. The vector ω shown speciﬁes the magnitude of angular velocity ω, the direction of the axis of rotation, and the sense of rotation. The velocity of point A speciﬁed by position vector r is then v = ω × (r − r0 )

(a)

ω

v

r – r0 P r0

O FIGURE 3.15 Angular velocity in rigid-body rotation.

© 2005 by Chapman & Hall/CRC Press

r

A

124

Continuum Mechanics and Plasticity

In the index notation, (a) is written as (0)

vi = eijk ωj (xk − xk )

(b)

From vector ω we deﬁne its dual tensor as jk = −eijk ωi

(c)

Substituting (c) into (b), we obtain (0)

vi = ik (xk − xk )

or

v = · (r − r0 )

(d)

We see that the angular velocity can be represented either by vector ω or tensor .

3.13

Velocity of a Particle Relative to a Neighboring Particle

We consider two particles P and P in a continuum in motion. The coordinate of P is XR initially, and xi at time t. For the sake of simplicity, the origins and axes of the material and spatial coordinate systems coincide. The coordinate of P is XR + XR initially, and xi + xi at time t. The line element between the two particles is dXR initially and dxi at time t. The initial and deformed line element are related by dxi =

∂xi dXR ∂XR

(3.159)

The relative velocity of P with respect to P is dvi ≡ vi (P , t) − vi (P, t) = vi (XR + dXR , t) − vi (XR , t) = v˜ i (xj + dxj , t) − v˜ i (xj , t)

(3.160)

in which the particle velocity is either expressed in the material description by the use of function vi (XR , t) or in the spatial description by the use of function v˜ i (xi , t). From the material description, (3.160) may be further written as dvi =

D [xi (XR + dXR , t) − xi (XR , t)] Dt

(3.161)

Observing that dxi denotes the line element connecting two adjacent material particles, (3.161) reduces to dvi =

© 2005 by Chapman & Hall/CRC Press

D (dxi ) Dt

(3.162)

Motion and Deformation

125

It is seen from (3.162) that the order of differentiation between d and D/Dt is interchangeable. Using the spatial description, from (3.160), we write dvi = v˜ i (xj + dxj , t) − v˜ i (xj , t)

(3.163)

The ﬁrst term on the right-hand side may be expanded in Taylor’s series and, by retaining only the ﬁrst-order term, (3.163) becomes dvi = v˜ i (xj , t) +

∂ v˜ i ∂ v˜ i dxk − v˜ i (xj , t) = dxk = vi,j dxj ∂xk ∂xk

(3.164)

Combining (3.162) and (3.164), we obtain dvi =

D(dxi ) = vi,j dxj Dt

(3.165)

where vi,j = Lij is known as the velocity gradient tensor. This tensor is generally not symmetric and so it can be split into symmetric and antisymmetric parts. Therefore, we write Lij = vi,j = 12 (vi,j + vj,i ) + 12 (vi,j − vj,i ) = Dij + Wij

(3.166)

where Dij = 12 (vi,j + vj,i )

or

D = 12 (L + LT )

(3.167)

Wij = 12 (vi,j − vj,i )

or

W = 12 (L − LT )

(3.168)

and

in which Dij is the rate of deformation tensor and Wij is the spin tensor. Therefore, (3.165) may be rewritten as dvi = Dij dxj + Wij dxj

3.14

(3.169)

Physical Signiﬁcance of the Rate of Deformation Tensor

In order to see the physical signiﬁcance of the rate of deformation tensor Dij , (1) (2) let us consider two material line elements, dxi and dxi , at the current conﬁguration in the spatial system. Let φ be the angle formed by the two line (1) (2) elements, with unit vectors ni and ni and lengths ds1 and ds2 , respectively.

© 2005 by Chapman & Hall/CRC Press

126

Continuum Mechanics and Plasticity (1)

(2)

We then differentiate the inner product dxi dxi to yield

of the two line elements

D (1) (2) (1) (2) (1) (2) (1) (2) dxi dxi = vi,j dxj dxi + dxi vi,j dxj = dxi dxj [vi,j + vj,i ] Dt (3.170) or D (1) (2) (1) (2) dxi dxi = 2Dij dxi dxj Dt (1)

(2)

On the other hand, since dxi dxi equation by differentiation,

(3.171)

= ds1 ds2 cos φ, we obtain the following

D D Dφ D (1) (2) dxi dxi = (ds1 )ds2 cos φ + ds1 (ds2 ) cos φ − ds1 ds2 sin φ Dt Dt Dt Dt (3.172) Equating (3.171) and (3.172), and dividing the resulting equation by ds1 ds2 , we obtain 1 D 1 D Dφ (1) (2) (ds1 ) cos φ + (ds2 ) cos φ − sin φ = 2Dij ni nj ds1 Dt ds2 Dt Dt

(3.173)

Note that ni = dxi /ds in the above equation. Special cases may be deduced from (3.173). If the two line elements coincide, then φ = 0 and ds1 = ds2 = ds. In this case, (3.173) reduces to 1 D (ds) = Dij ni nj ds Dt

(3.174)

The expression on the left-hand side of (3.174) is precisely the deﬁnition of true strain-rate, which is the rate of length change per unit length at the current conﬁguration. Knowing Dij and specifying a direction ni , the strainrate along this direction may be found from (3.174). Using the concept of stretch ratio λ = ds/dS, where dS does not change with time, (3.174) may be expressed as λ˙ = Dij ni nj λ

(3.175)

In particular, let ni = (1, 0, 0), then (1/ds1 )((D/Dt)ds1 ) = λ˙ 1 /λ1 = D11 , where D11 is time rate of change (extension or contraction) per unit length of an element, which at time t is oriented along the x1 axis. A similar interpretation applies to D22 and D33 .

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

127

To see the physical meaning of the off-diagonal terms of the Dij matrix, let φ = 90◦ in (3.173). Then, the two line elements are perpendicular to each other at time t. In this case, (3.173) reduces to − (1)

In particular let ni

Dφ (1) (2) = 2Dij ni nj Dt (2)

be along the x1 axis and ni −

(3.176) be along x2 , then

Dφ = 2D12 Dt

(3.177)

It is seen that D12 is the shear rate. The quantity −Dφ/Dt is the rate of change (1) (2) of the right angle between the two elements dxi and dxi . The negative sign means that the angle φ is decreasing. If we let θ = 90◦ − φ, then Dθ/Dt = −Dφ/Dt, that is, θ is increasing. A similar interpretation applies to D13 and D23 . Show that the necessary and sufﬁcient condition for rigidbody motion of a continuum is Dij = 0.

EXAMPLE 3.7

Proof The length ds of a deformed line element is ds2 = dxi dxi

(a)

Material differentiation of (a) yields D D D (ds2 ) = (dxi dxi ) = 2 (dxi )dxi = 2vi,j dxj dxi Dt Dt Dt

(b)

where we used (3.165). We observe that the last expression of (b) is symmetric in i and j and it may be further written as D (ds2 ) = (vi,j + vj,i )dxi dxj = 2Dij dxi dxj Dt

(c)

In (c), dxi is a vector connecting two neighboring points and it is arbitrary and nonzero. The quantity D(ds2 )/Dt is 0, if and only if Dij = 0. But D(ds2 )/Dt = 0 implies that the length of an arbitrary line element in a body does not change, which precisely is the deﬁnition for a rigid body.

© 2005 by Chapman & Hall/CRC Press

128

3.15

Continuum Mechanics and Plasticity

Physical Signiﬁcance of the Spin Tensor

Consider a pure rigid-body rotation, which is a special case of motion of a continuum. Let the motion be described by xi = QiR (t)XR

(3.178)

where QiR is a function of time t and is orthogonal such that QiR (t)QjR (t) = δij ,

QiR (t)QiS (t) = δRS ,

and |QiR | = 1

(3.179)

Differentiating (3.178) with respect to time, we obtain ˙ iR XR vi = Q

˙ iR = d QiR where Q dt

(3.180)

In the above expression, the velocity is expressed in the material system XR that does not change with time. On the other hand, the velocity may be expressed in the spatial description. To show this, we invert (3.178) to yield XR = QjR xj

(3.181)

By substitution, we obtain from (3.180) and (3.181) ˙ iR QjR xj vi = Q

(3.182)

We see that the velocity is in the spatial description in (3.182). If we differentiate the ﬁrst equation of (3.179), we ﬁnd ˙ iR QjR = −QiR Q ˙ jR ij = Q

(3.183)

From (3.183), we see that the quantity ij is antisymmetric. Substituting this result back into (3.182), we ﬁnd that rigid-body rotation of a continuum is governed by the following velocity ﬁeld vi = ij (t)xj

(3.184)

At any instant of time t, the increment of (3.184) can be compared with (3.165) and (3.169). This can be seen in the case of rigid-body rotation Lij = Wij = ij and Dij = 0, where the spin tensor can be identiﬁed with the angular velocity of the rigid-body motion. The angular velocity tensor ij is further related to the velocity gradient through (3.168). Since ij is antisymmetric, it has only

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

129

three nonzero independent components in the off-diagonal terms. In terms of the dual vector ωk as in (3.158), the matrix of ij is

ω2 −ω1 0

−ω3 0 ω1

0 ij = ω3 −ω2

(3.185)

Also, using (3.157), we form eijm ij = −eijm eijk ωk = −2δmk ωk

(3.186)

ωk = − 12 eijk ij

(3.187)

or

Substituting (3.157) into (3.184), the particle velocity is now given by vi = −eijk ωk xj = ekji ωk xj

or

v =ω×x

(3.188)

where ω is the angular velocity vector of the rigid-body rotation. We note that in a general motion of a continuum, W is not equal to and is determined by (3.168), expressed in terms of velocity gradients. The dual vector of W is given by wk = − 12 eijk 21 (vi,j − vj,i ) = − 12 eijk vi,j = 12 ejik vi,j

(3.189)

or w=

1 2

Curl v

(3.190)

This is the vorticity vector, which is frequently used in ﬂuid mechanics.

3.16

Expressions for D and W in Terms of F

Although (3.167) and (3.168) may be used to describe a continuum undergoing general motions, we derive here the expressions of D and W in terms of the deformation gradient F. We do this because F has been used extensively in the description of deformation. The velocity gradient L may be written as L=

∂v ∂v ∂X = · = F˙ · F−1 = −F · (F−1 )· ∂x ∂X ∂x

© 2005 by Chapman & Hall/CRC Press

(3.191)

130

Continuum Mechanics and Plasticity

where the last equality has been obtained from the differentiation of F · F−1 = 1. If we use the right polar decomposition of F given by (3.26), then (3.191) becomes L = −(R · U) · ((R · U)−1 )· = −R · U · (U−1 · R−1 )· = −R · U · [(U−1 )· · R−1 + U−1 · (R−1 )· ] = −R · U · (U−1 )· · RT − R · R˙ T ˙ · U−1 · RT + R ˙ · RT =R·U

(3.192)

In the derivation of (3.192), we recognized the relation R−1 = RT and used the results obtained from the differentiation of relations U · U−1 = 1 and R · RT = 1. We now take the transpose of (3.192) to yield ˙ · U−1 )T + (R ˙ · R T )T LT = R · (R · U

(3.193)

Therefore, from (3.192) and (3.193), we obtain ˙ · U−1 + U−1 · U) ˙ · RT D = 12 (L + LT ) = 12 R · (U

(3.194)

and ˙ · U−1 − U−1 · U) ˙ · RT + R ˙ · RT W = 12 (L − LT ) = 12 R · (U

(3.195)

Similarly, by use of the left polar decomposition (3.27), we may show that ˙ · V−1 + V−1 · V ˙ +V·R ˙ · RT · V−1 − V−1 · R ˙ · RT · V) D = 12 (V

(3.196)

and ˙ · V−1 − V−1 · V ˙ +V·R ˙ · RT · V−1 + V−1 · R ˙ · RT · V) W = 12 (V

(3.197)

Show that the spin tensor W describes the angular velocity of the principal axes of the rate of deformation tensor D.

EXAMPLE 3.8

Proof Let ni be a normalized eigenvector of Dij and ni = dxi /ds. We take the material derivative of ni and write D n˙ i = Dt

dxi ds

= vi,j nj −

=

dxi 1 D 1 1 D 1 D (dxi ) − 2 (ds)dxi = vi,j dxj − (ds) ds Dt ds ds Dt ds ds Dt

λ˙ ni = vi,j nj − Djk nj nk ni = (Dij + Wij )nj − Djk nj nk ni λ

© 2005 by Chapman & Hall/CRC Press

(a)

Motion and Deformation

131 D (ds)/dS and Dt (for p = 1, 2, 3) the eigenvectors of Dij , we write

Note that, in the derivation of (a), we used λ = ds/dS, λ˙ = (p)

(3.175). Denoting by ni

(p)

(Dij − D(p) δij )nj

=0

(b)

where D(p) is the corresponding principal value of Dij . Using (b), we replace (p)

(p)

(p) (p)

Dij nj by D(p) ni , and using relation ni nj may be written as (p)

n˙ i

(p)

= D(p) ni

(p)

+ Wij nj (p)

= −eijm wm nj

= δij given by (2.86), equation (a) (p) (p) (p)

− D(p) nk nk ni (p)

= eijk wj nk

(p)

= Wij nj

(c)

In the symbolic notation, (c) is written as n˙ (p) = w × n(p)

(d)

This expression shows that w is the angular velocity of n(p) , which is a principal direction of the rate of deformation tensor D.

3.17

Material Derivative of Strain Measures

We introduced several strain measures in earlier sections of this chapter. In this section, we explore the relationships between the material derivatives, denoted by a dot, of C and E and the rate of deformation D. Let us differentiate (3.40) ﬁrst to obtain ∂xi ∂vi ∂vi ∂xi ∂xi ∂vi ∂xk ∂vi ∂xk ∂xi C˙ RS = + = + ∂XR ∂XS ∂XR ∂XS ∂XR ∂xk ∂XS ∂xk ∂XR ∂XS ∂vi ∂xi ∂xk ∂vk ∂xi ∂xk = + = 2Dik (3.198) ∂xk ∂xi ∂XR ∂XS ∂XR ∂XS We then differentiate (3.100) and ﬁnd 2E˙ RS = C˙ RS

(3.199)

Summarizing (3.198) and (3.199), we have ∂xi ∂xk 1 E˙ RS = C˙ RS = Dik 2 ∂XR ∂XS

(3.200)

Equation (3.200) relates the material derivatives E˙ RS and C˙ RS to the rate of deformation Dij .

© 2005 by Chapman & Hall/CRC Press

132

Continuum Mechanics and Plasticity

EXAMPLE 3.9

Show that the material derivative of the Jacobian is given by DJ ∂vk =J Dt ∂xk

(a)

Proof DJ D|∂xi /∂XR | ∂J ∂J D(∂xk /∂XS ) ∂vk ∂xm = = = Dt Dt ∂(∂xk /∂XS ) Dt ∂(∂xk /∂XS ) ∂xm ∂XS Using (2.76), the expression ∂J/∂ and according to (2.84), we write

∂xk ∂XS

in (b) is the cofactor of matrix

∂J ∂XS =J ∂xk ∂(∂xk /∂XS )

(b) ∂xk ∂XS ,

(c)

Substituting (c) into (b), we obtain (a).

3.18

Material Derivative of Area and Volume Elements

We ﬁrst ﬁnd the material derivative of an area element. The deformed and initial areas are related by Nanson’s formula (3.92), and the differentiation of (3.92) leads to D DJ ∂XR D D ∂XR ∂XR (dai ) = dAR dAR = +J J Dt Dt ∂xi Dt ∂xi Dt ∂xi

(3.201)

Deriving an expression to represent the last term of (3.201), we differentiate the expression ∂xi ∂XR = δij ∂XR ∂xj

(3.202)

to obtain D Dt

∂xi ∂XR

∂XR ∂xi D + ∂xj ∂XR Dt

∂XR ∂xj

=0

(3.203)

This equation may be further simpliﬁed to yield ∂vi ∂xi D + ∂xj ∂XR Dt

© 2005 by Chapman & Hall/CRC Press

∂XR ∂xj

=0

(3.204)

Motion and Deformation

133

which reduces to D Dt

∂XR ∂xj

=−

∂vi ∂XR ∂xj ∂xi

(3.205)

Substituting (3.205) and the expression of Example 3.9 into (3.201) to obtain D (dai ) = Dt

=J

DJ ∂XR D +J Dt ∂xi Dt

∂XR ∂xi

dAR

∂vk ∂XR ∂vk ∂XR ∂vk ∂vk dAR − J dAR = dai − dak ∂xk ∂xi ∂xi ∂xk ∂xk ∂xi

(3.206)

we may conclude that the material rate of an area element is D ∂vk ∂vk (dai ) = dai − dak Dt ∂xk ∂xi

(3.207)

Finally, let us consider the material derivative of the volume element. Since dV = J dV0 , we can differentiate the equation to obtain D(dV) D DJ ∂vk ∂vk = (JdV0 ) = dV0 = J dV0 = dV = Dkk dV Dt Dt Dt ∂xk ∂xk

(3.208)

The material derivative of the logarithmic volumetric strain is then D 1 D(dV) [ln(dV)] = = vk,k = Div v = Dkk Dt dV Dt

(3.209)

All of the last three forms in (3.209) have been used in the continuum mechanics literature. When there is no volume change, we have from (3.208) or (3.209), vk,k = Dkk = Div v = 0. This is a necessary and sufﬁcient condition for the material element to undergo no volume change. We note that a material element undergoing no volume change is merely a geometrical condition. It has no implication as to whether the material is compressible or not. But, when a material element does not suffer any volume change in all loading conditions, the material is then incompressible.

References 1. Truesdell, C. and Toupin, R. S. Flugge (ed.) The Classical Field Theories, in Handbuch der Physik, Vol. III/1, Springer-Verlag, Berlin, 1960. 2. Spencer, A.J.M., Continuum Mechanics, Longman, London and New York, 1980. 3. Chadwick, P., Continuum Mechanics, George Allen & Unwin, London, 1976. 4. Eringen, A.C., Mechanics of Continua, Wiley, New York, 1967.

© 2005 by Chapman & Hall/CRC Press

134

Continuum Mechanics and Plasticity

Problems (1) In the deformation deﬁned by x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

ﬁnd the expressions for the following tensors: F, C, U, R, where λi are constants. If λ1 = 1.2, λ2 = 0.8, and λ3 = 1, sketch the deformed shape of a unit cube. (2) In the deformation of problem 1 with λ1 = 1.2, λ2 = 0.8, and λ3 = 1, determine the deformed length of a diagonal connecting point O (0, 0, 0) to point C (1, 1, 1). Determine also the ﬁnal orientation of this diagonal. (3) Consider the following deformation and refer to Figure 3.16 x1 = λ1 X1 + X2 tan γ ,

x2 = λ2 X2 ,

x3 = λ3 X3

where λi and γ are constants. Sketch the deformed shape of square OABC in the X1 − X2 plane. The sides are initially of unit length.

X2

C

O

B

A

X1

X3 FIGURE 3.16

(4) For the simple shearing deformation given by x1 = X1 +kX2 , x2 = X2 , x3 = X3 , where k is a constant, ﬁnd the components of C in terms of k and determine the eigenvalues and eigenvectors of C. Discuss the eigenvalues and eigenvectors of C as k varies from negative to positive and from small to large values. (5) For the simple shearing deformation given by x1 = X1 +kX2 , x2 = X2 , x3 = X3 , where k is a constant, represent by a sketch the deformed area to which the

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

135 X3

C (0, 0, 1)

B (0,1,0)

O

(1, 0, 0)

X2

A

X1 FIGURE 3.17

original area OABC transforms (see Figure 3.17). Obtain an expression to describe the direction of the line element OA after deformation. (6) Consider the following deformation x1 =

√ 2X1 + 43 X2 ,

x2 = X1 − 43 X2 + 41 X3 ,

x3 =

√ 2X3

Find (a) the direction after the deformation of a line element, which is initially oriented with a direction ratio 1:1:1; (b) the stretch ratio of this line element. (7) By use of the imaging-based method, the locations of the four corners of a twodimensional, initially square, material element have been determined after deformation. The initial and deformed elements are shown in Figure 3.18. Using the property that F transforms undeformed line elements into deformed line elements, determine the components of F and C.

D (0, 1)

C⬘ (1.3, 1.1) D⬘ (0.5, 0.9)

C (1, 1)

(0.8, 0.2) B⬘ A (0, 0) FIGURE 3.18

© 2005 by Chapman & Hall/CRC Press

B (1, 0)

136

Continuum Mechanics and Plasticity X3

A

O

B

X2

D

C

X1 FIGURE 3.19 Figure for Problem 11.

(8) Show that

cos θ FiR = sin θ 0

− sin θ cos θ 0

0 0 1

describes a rigid-body rotation. (9) A square element is subjected to a uniaxial extension in the 1 direction, and is then rotated about the positive 3 direction through an angle of 90◦ . Determine the deformation gradient F. (10) In the case of plane strain, experimental measurements give stretch ratios λ of 0.8 and 1.2 in the X1 and X2 directions, respectively, and 0.6 in the direction making a 45◦ angle with the X1 axis. Determine the components of C and E. (11) Consider the unit cube shown in Figure 3.19, which undergoes the deformation x1 = α X1 − 12 X2 ,

x2 = βX2 ,

x3 = γ X3

where α, β, and γ are constants. Determine (a) the deformed length of diagonal OA (b) the angle between OB and OD after deformation (c) the condition that constants α, β, and γ must satisfy if the material is incompressible. (12) For the deformation of Problem (11), determine the expressions for components of tensors F, C, U, V, R, B, E, and e. Use α = 1.2, β = γ = 0.9.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

137

(13) In the case of simple shear deformation of a square block governed by x1 = X1 + kX2 ,

x2 = X2 ,

x3 = X3

where k is constant, determine the extension ratios for the sides and the diagonals. Find the volume of the block before and after deformation. (14) The most general two-dimensional homogeneous deformation is deﬁned by the following linear transformation x1 = aX1 + bX2 ,

x2 = cX1 + dX2 ,

x3 = X3

Find components of C, B, and E in terms of constants a, b, c, and d. (15) Consider the following deformation and refer to Figure 3.16 x1 = X1 + 12 X22 ,

x2 = X2 ,

x3 = X3

(a) Sketch the deformed shape of square OABC in the X1 − X2 plane. The sides are initially of unit length. (b) Consider at point O two line elements: dX(1) = dX(1) e1 and dX(2) = dX(2) e2 . Find the deformed line elements dx(1) and dx(2) , and calculate the dot product dx(1) · dx(2) . Determine the change in the original right angle between dX(1) and dX(2) due to deformation. (c) Do the same thing as in (b) for two line elements dX(1) = dX(1) e1 and dX(2) = dX(2) e2 located at point C. (16) In the initial conﬁguration, a circular cylinder with radius R has its axis aligned with the X3 direction. If the cylinder undergoes the deformation x1 = α{X1 cos(τ X3 ) + X2 sin(τ X3 )} x2 = α{−X1 sin(τ X3 ) + X2 cos(τ X3 )} x3 = βX3 determine the conditions that need to be satisﬁed by constants α, β, and τ so that the volume is preserved during deformation. Determine the length of a line element in the deformed conﬁguration, which initially has unit length and lies on the surface of the cylinder along the X3 direction. Determine also the initial length of a line element on the surface of the cylinder that, in the deformed conﬁguration, has unit length and lies in the X3 direction. (17) For an isotropic material, the coefﬁcient of thermal expansion is αij = αδij , where α is a constant. A line element of length L elongates an amount dL if the temperature is raised by dT, so that dL = αdTL. For a block of L1 × L2 × L3 subjected to this change in temperature, write down the set of three transformation equations that describes this deformation. Find the components of F and determine the current length of a diagonal of the block, which had an initial length of L.

© 2005 by Chapman & Hall/CRC Press

138

Continuum Mechanics and Plasticity

(18) If the eigenvalues for U are λ(i)• = 3, 13 , 1 and the corresponding eigenvectors are

√

√ 3 3 1 1 (1)T (2)T (3)T nu = , ,0 , nu = − , ,0 , nu = (0, 0, 1) 2 2 2 2 use E = f(U) =

i

(i)

(i)

f (λi )nu ⊗ nu with f (λi ) =

λκi −1 to determine the κ

components of E with respect to the XR system when κ = 2 and −2. (19) If the eigenvalues for V are λ(i) = 3, 13 , 1 and the corresponding eigenvectors are

√

√ 1 3 1 3 (1)T (2)T (3)T nv = , , 0 , nv = − , , 0 , nv = [0, 0, 1] 2 2 2 2 (i) (i) use e = f(V) = i f (λi )nv ⊗nv with f (λi ) = (λκi −1)/κ to determine the components of e with respect to the xi system when κ = 2 and −2. Assume that XR and xi coincide for simplicity. (20) Consider a rectangular triad before deformation. Discuss what would happen to this triad after deformation. Would it remain rectangular? Under what condition? (21) Let the displacement ﬁeld be given by u1 = 41 (X3 − X2 ),

u2 = 41 (X1 − X3 ),

u3 = 41 (X2 − X1 )

Determine the volume ratio dV/dV0 . (22) Show that the velocity ﬁeld v1 = 2x3 − 3x2 ,

v2 = 3x1 − x3 ,

v3 = x2 − 2x1

corresponds to a rigid-body rotation. Determine this rotation by a vector so that we know the axis of rotation. (23) Consider the motion x1 = X1 + 12 X22 t,

x2 = X2 ,

x3 = X3

At t = 0, the corners of a unit square are at O (0, 0, 0), A (1, 0, 0), B (1, 1, 0), and C (0, 1, 0). Sketch the deformed shape of square OABC in the X1 − X2 plane when t = 1 and when t = 2. (24) For the motion of Problem (23), determine the velocity and acceleration of a particle in both material and spatial descriptions. (25) For the motion of Problem (23), determine the expressions for L, D, and W. (26) For the velocity ﬁeld v1 = −αx2 , v2 = αx1 , v3 = β, where α and β are constants, ﬁnd the components of tensors L, D, and W.

© 2005 by Chapman & Hall/CRC Press

Motion and Deformation

139

(27) Let a velocity ﬁeld be described by vi = αxj µi vj , where the scalar α and the orthogonal unit vectors µ and ν are independent of the coordinate xi . Show that this velocity ﬁeld represents simple shearing. Find the principal values and directions of the rate of deformation D with respect to the directions of µ and ν. (28) Prove that, if the Dij components of a velocity ﬁeld are independent of the coordinates and the principal invariants ID and III D are both 0, the velocity ﬁeld represents simple shearing. (29) Consider the motion x1 = X1 + kX22 t2 ,

x2 = (1 + kt)X2 ,

and

x3 = X3

where k is a constant and the material coordinate XR designates the position of a particle at t = 0. (a) At t = 0 the corners of a unit square are at O (0, 0, 0), A (0, 1, 0), B (1, 1, 0), and C (1, 0, 0). Sketch the shape of the square at t = 1.5. (b) Obtain the spatial description of the velocity and acceleration ﬁelds. (c) Obtain the expressions for the rate of deformation D and the spin tensor W. (d) What happens to the volume of an inﬁnitesimal element located initially at (0.6, 0.5, 1)? (30) In the motion of a continuum, the velocity of a particle is given by v1 = (x12 + x1 x2 )e−kt ,

v2 = (x22 − x1 x2 )e−kt ,

v3 = 0

where k is a constant and t is time. Determine the following properties at point (1, 1, 1) when t = 0: (a) the principal values of the rate of deformation D, (b) the maximum shear rate. (31) For the motion of Problem (30), determine the volumetric strain-rate deﬁned by (1/dV)((D(dV))/Dt), where dV is the current volume of an element. (32) The velocity ﬁeld of a continuum is prescribed by v1 = f (x2 ) − x2 g(r),

v2 = x1 g(r),

v3 = 0

with r = (x12 + x22 )1/2

Determine the rate of deformation D and the vorticity vector w, which is the dual vector of the spin tensor W. Discuss the type of motion that the continuum is undergoing. (33) Let the components of D be

α [D] = β β

© 2005 by Chapman & Hall/CRC Press

β α β

β β α

140

Continuum Mechanics and Plasticity Consider a line element with direction denoted by the unit vector n. If the rate of extension of the line element is α, ﬁnd the condition that the components of n must fulﬁll.

(34) Consider the motion of a deformable element. Do all line elements in Figure 3.20 spin with the same angular velocity? The spin of which line element does the spin tensor W describe? x2

B

F

C G

A FIGURE 3.20

© 2005 by Chapman & Hall/CRC Press

D

x1

4 Conservation Laws and Constitutive Equation

4.1

Introduction

This chapter discusses the governing equations of a body undergoing deformation. The equations include the conservation laws of physics and the constitutive equations. The conservation laws of physics are the conservation of mass, linear momentum, angular momentum, and energy. These laws are ﬁrst developed in the global form and then reduced to the local form. The global form considers forces, momentum, or energy acted on the whole deformable body, whereas the local form refers to a generic inﬁnitesimal element of the body. The conservation laws are applicable to a body of any material. To distinguish between deformation of a body made of different materials, we need constitute equations. As an example, let us consider applying a tensile force to a long bar. The conservation laws for the problem are the same no matter what material the bar is made of. However, experiments show that long bars made of wood or steel will undergo different amounts of deformation when subjected to the same tensile force. Therefore, in order to accurately describe the elongation of the bars, we need to introduce constitutive equations, which accurately represent the two different materials of the bars, that is, we need a constitutive equation of for wood and another for steel. Constitutive equations are a set of equations, which describe the thermomechanical properties of a material. Depending on the simplicity/complexity of the material behavior that we wish to describe, we may need one constitutive equation or a set of constitutive equations. Hooke’s law is the most well-known constitutive equation for solids, and it is also the simplest form that a constitutive equation for solid can have. However, there is a limitation to the validity of Hooke’s law. It is usually applicable when the deformation is small and linearly elastic at room temperature. The equation needs to be modiﬁed or extended to a set of (nonlinear) equations when the deformation is large and nonelastic and not at constant temperature. Hooke’s law is also known as the stress–strain relation, because the equation relates the stress to the strain; for isotropic linearly elastic solid, it is 141

© 2005 by Chapman & Hall/CRC Press

142

Continuum Mechanics and Plasticity

written as σ = 2µε + λIεkk

(4.1)

where σ and ε are the engineering stress and strain, respectively, and µ and λ are the Lamé constants.‘ The effect of temperature on the material behavior is not discussed in this chapter. Even at constant temperature, the material behavior of a real material can be quite complex. Realistic constitutive equations should be used in order to obtain useful solutions of engineering problems. In addition to the elastic behavior, some materials exhibit strong viscous behaviors and some are signiﬁcantly inﬂuenced by plastic deformation. The viscous behaviors are observable in the forms of the strain-rate effect, creep and stress relaxation. These behaviors are usually discussed within the contest of viscoelasticity and viscoplasticity. The viscoplastic behavior is discussed in Chapter 5. The subject of plastic deformation is one of the main topics of this book and is thoroughly discussed in the later part of the book. In this chapter, we ﬁrst derive the conservation equations. The bulk material rate of change is discussed. This is useful in the derivation of the conservation laws in the global form. In the local form, we derive the conservation equations for an inﬁnitesimal material element at the deformed conﬁguration. This is a spatial description. We then discuss the material description of the conservation laws, which leads to the discussion of several stressmeasures, referring to the deformed or undeformed conﬁgurations. In the topics related to constitutive equations, we ﬁrst discuss the general principles, including the principle of material objectivity. We then derive the constitutive equation for large elastic deformation, which include different types of formulations. Emphasis is placed upon hyperelasticity and some examples are given. Finally, the generalized Hooke’s law for inﬁnitesimal elastic deformation is discussed.

4.2

Bulk Material Rate of Change

We discuss the bulk material rate here, because it is useful when we consider the global form of the conservation laws in the next section. The bulk material rate is the material rate of change of a physical property deﬁned over a material body. Referring to Figure 4.1, we let the material body occupy the space shown by the solid line at time t and let the body occupy the space shown by the dashed line at time t + t. The volume and surface of the body at t and t + t are (V, S) and (V , S ), respectively. Let φ(xi , t) be a property of the continuum, which is a tensor quantity. Considering the volume integral I= © 2005 by Chapman & Hall/CRC Press

V

φ dV

(4.2)

Conservation Laws and Constitutive Equation

143

∆V2 vdt S2 dS xi dS

vdt

n x3 x2

S1

xi + vi dt = xi + ∆xi n

V ⬘, S⬘ (at t + ∆t)

∆V1

V, S (at t) x1 FIGURE 4.1 Bulk material rate of change.

we are then interested in ﬁnding the derivative DI/Dt. To ﬁx ideas, let us assume that φ = ρ(xi , t) is the density of the continuum, then the integral I = V ρ dV is the total mass of the body. The derivative of (4.2) is

φ(xi + xi , t + t)dV − V φ(xi , t)dV] t [ V φ(xi , t + t)dV − V φ(xi , t)dV] = lim t→0 t [ V φ(xi + xi , t + t)dV − V φ(xi , t + t)dV] + lim t→0 t

[ DI = lim Dt t→0

V

(4.3)

In the second equality of (4.3), the term V φ(xi , t + t)dV has been added and subtracted. We now ﬁnd physical interpretations for the terms of (4.3). Letting V = υ + V1 , V = υ + V2 , then υ is the common volume of V and V and is denoted by the shaded area in Figure 4.1; V1 is the volume in V and V2 is the volume in V both of which are denoted by the moon-shaped area. Equation (4.3) may be interpreted as DI (Total mass in V at t + t − Total mass in V at t) = lim Dt t→0 t (Total mass in V at t + t − Total mass in V at t + t) + lim t→0 t = (Rate of increase of mass in ﬁxed region V) (Total mass in V2 at t + t − that in V1 at t + t) t→0 t

+ lim

© 2005 by Chapman & Hall/CRC Press

(4.4)

144

Continuum Mechanics and Plasticity

where the last term is the net amount of mass increased in V per unit time. Equation (4.3) may then be written as ( V2 φ dV − V1 φ dV) ∂φ dV + lim t→0 t V ∂t [ φvt · n dS + S1 φvt · (n dS)] ∂φ S2 = dV + lim t→0 t V ∂t

DI = Dt

(4.5)

Note that the surface S of the body at time t is seen in Figure 4.1 to be divided into S1 and S2 so that S = S1 + S2 . A particle on the surface S2 has coordinates xi with velocity v, and the particle moves to a new position xi + xi during the time interval t, and we write xi + vi t = xi + xi . Denoting the area element at this particle by dS and its unit normal by n, we observe that this area element sweeps through a volume V = vt · ndS during the time interval t, and area S2 sweeps through volume V2 . The same thing may be said of particles on surface S1 , except that the scalar product V = vt · ndS is negative. This may be seen from Figure 4.1, because vectors n and v form an obtuse angle. Thus, during time interval t, surface S1 sweeps through volume V1 . The two integrals within the parenthesis in (4.5) can then be added to form one integral and the equation becomes ∂φ ∂φ dV + φvi ni dS = dV + (φvi ),i dV V ∂t S V ∂t V ∂φ + φ,i vi + φvi,i dV = ∂t V

DI = Dt

(4.6)

The Gauss theorem discussed in Section 1.8.3 was used in the derivation of (4.6), which may be further written as D Dt

V

φ dV =

V

Dφ + φvi,i dV Dt

(4.7)

This is the material derivative of the integral of a property φ deﬁned over volume V. We used φ = ρ in the above derivation for easy interpretation, but (4.7) is valid for any scalar property of the material. We now consider an alternative derivation of (4.7). Let I = I(t) which, in general, is a function of time and we write I=

V

φ dV =

V0

φ(XR , t) det F dV0

(4.8)

In arriving at the last equality of (4.8), (3.82) and the coordinate transformation XR = XR (xi , t) was applied. Noting that V0 is time independent, we

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation differentiate (4.8) to obtain DI Dφ D = det F + φ (det F) dV0 Dt Dt V0 Dt

145

(4.9)

To further reduce equation (4.9) to a simple form, we apply the following expression that was deduced in Example 3.9 DJ ∂vk =J Dt ∂xk

(4.10)

Note that J = det F. Using (4.10), (4.9) becomes DI = Dt

V0

Dφ Dφ det F + φ det F vi,i dV0 = + φvi,i det F dV0 (4.11) Dt V0 Dt

Therefore, we may conclude that DI = Dt

V

Dφ + φvi,i dV Dt

(4.12)

which is the same as (4.7).

4.3

Conservation Laws

There are three conservation laws from physics, and they are valid for all materials. They are: (i) the conservation of mass, (ii) the conservation of momentum, and (iii) the conservation of energy. These laws are discussed individually and written in mathematical expressions in this section.

4.3.1

The Conservation of Mass

The mass of a body is preserved when only thermo-mechanical behavior is being considered. In this case, the rate of change of mass is zero. Setting φ = ρ in (4.2), the integral I is the mass of the body. The global form of the conservation of mass is written as D ρ dV = 0 (4.13) Dt V Using (4.7), (4.13) may be further written as D Dt

© 2005 by Chapman & Hall/CRC Press

V

ρ dV = 0 =

V

Dρ + ρvi,i dV Dt

(4.14)

146

Continuum Mechanics and Plasticity

which must be true for all volume elements. Thus, the local form (or differential form) of the conservation of mass is Dρ + ρvi,i = 0 Dt

(4.15)

Dρ ∂ρ(xi , t) ∂ρ vj = + Dt ∂t ∂xj

(4.16)

∂(ρvi ) ∂ρ =0 + ∂t ∂xi

(4.17)

But, since

we obtain from (4.15)

Equation (4.17) is known as the continuity equation in ﬂuid mechanics.

4.3.2

The Conservation of Momentum

We need to consider both the conservation of linear momentum and angular momentum. The rate of change of linear momentum is equal to the resultant force and the conservation equation is D Dt

V

ρvi dV =

V

bi dV +

(n)

S

ti

dS

(4.18)

Equation (4.18) is the conservation of linear momentum in the global form. The left-hand side of (4.18) is the rate of change of linear momentum. The ﬁrst term on the right-hand side is the total body force and the second term is the total surface traction. Using (2.8) and an identity proven in Example 4.1, (4.18) may be written as

D bi dV + σki nk dS = Dt V S

V

ρvi dV =

V

ρ

Dvi dV Dt

(4.19)

or, by use of the Gauss theorem, we obtain V

bi + σki,k − ρ

Dvi Dt

dV = 0

(4.20)

In the local form, (4.20) reduces to σki,k + bi = ρ which is known as the equation of motion.

© 2005 by Chapman & Hall/CRC Press

Dvi Dt

(4.21)

Conservation Laws and Constitutive Equation

147

The conservation of angular momentum states that the rate of change of the angular momentum is equal to the sum of moments of forces acting on the body. This law leads to the symmetry of stress tensor and has been discussed in Section 2.6 for the case when material element is in equilibrium. In the case of material element in motion, we have D (n) ρeijk xi bj dV + eijk xi tj dS = ρeijk xi vj dV (4.22) Dt V V S The ﬁrst term on the left-hand side of (4.22) denotes the moment due to the body force, the second term denotes the moment due to surface traction, and the term on the right-hand side denotes the rate of change of the angular momentum. Using (2.8) and the Gauss theorem, (4.22) is written as V

ρeijk xi bj +

D ∂ (eijk xi σmj ) dV = ρeijk (xi vj ) dV ∂xm Dt V Dvj = ρeijk vi vj + xi dV Dt V

(4.23)

in which ρeijk vi vj = 0. Hence, Dvj eijk xi σmj,m + bj − ρ dV + eijk σji dV = 0 Dt V V

(4.24)

By use of the equation of motion (4.21), the ﬁrst integral of (4.24) vanishes, and therefore, eijk σij = 0

(4.25)

σij = σji

(4.26)

which leads to

using an argument similar to that used in Section 2.6. Thus, we have shown that the conservation of angular momentum leads to the symmetry of the stress tensor for a body in motion. EXAMPLE 4.1 Show that D/Dt V ρφ dV = V ρ(Dφ/Dt) dV, where φ is a physical property deﬁned in V. Proof From (5.7), we have D D Dρ Dφ (ρφ)dV = (φρ) + φρvi,i dV = + ρvi,i + ρ dV φ Dt Dt Dt Dt V (a)

© 2005 by Chapman & Hall/CRC Press

148

Continuum Mechanics and Plasticity

In the last equality, Dρ/Dt + ρvi,i = 0 due to conservation of mass. Hence, (a) reduces to D Dt

4.3.3

V

ρφ dV =

V

ρ

Dφ dV Dt

(b)

The Conservation of Energy

The law of conservation of energy is the ﬁrst law of thermodynamics. According to this law, the sum of material derivatives of the internal and kinetic energies is equal to the sum of the rate of work of body and surface forces plus all other energies that enter the body per unit time. Other energies may include thermal, electrical, magnetic, or chemical energies. In this elementary text, we consider only the thermal energies and write DE DK DW DQ + = + Dt Dt Dt Dt

(4.27)

The equation is now explained term by term. E denotes the internal energy of the material element and is an extensive quantity, that is, an internal energy density ε may be deﬁned either per unit volume or per unit mass. In the case that ε is deﬁned per unit mass, we write E=

V

ρε dV

(4.28)

An extensive quantity is doubled if the mass or volume is doubled. On the other hand, the density cannot be deﬁned for an intensive quantity. Examples of intensive quantities are temperature and pressure. The internal energy includes all forms of energy in a system other than kinetic energy and potential energy. It represents energy modes on the microscopic level such as energy associated with nuclear spin, molecular binding, molecular translation and rotation, and molecular vibration, etc. The kinetic energy is related to the motion of the macroscopic element and is written as 1 K= ρvi vi dV (4.29) 2 V The second term in (4.27) is the rate of change of the kinetic energy and the third term is the rate of work due to external forces and is written as DW (n) = bi vi dV + ti vi dS (4.30) Dt V S and the last term of (4.27) is the rate of heat supply.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

149

There are two categories of heat supply: the heat ﬂowing across the boundary and the heat source. The heat ﬂowing through area element dS is −hi ni dS, where hi is the heat ﬂux vector and the direction of hi is the direction of the heat ﬂow. The magnitude of hi is the amount of heat per unit time per unit area normal to thedirection of heat ﬂow. Therefore, the part of DQ/Dt due to conduction is − S hi ni dS. We note that heat ﬂowing into the volume element is considered positive. Since the angle between hi and ni is obtuse, the negative sign is needed to make the heat ﬂow positive. The part of DQ/Dt due to distributed heat sources is D/Dt V ρq dV; where q is the heat supply per unit mass. Hence, the equation of conservation of energy in the global form, (4.27), may be written as D Dt

1 D ρε dV + ρvi vi dV Dt V V 2 D (n) = bi vi dV + ti vi dS − hi ni dS + ρq dV Dt V V S S

(4.31)

Using the result of Example 4.1, (4.31) becomes Dvi Dε ρvi dV + dV Dt Dt V V Dq = (σki vi ),k dV + bi vi dV − hi,i dV + ρ dV V V V V Dt

ρ

(4.32)

The ﬁrst integral on the right-hand side of (4.32) is

V

(σki vi ),k dV =

V

(σki,k vi + σki vi,k ) dV

(4.33)

Then, by use of the equation of motion (4.21), the energy balance equation may be simpliﬁed. Hence, (4.32) reduces to ρ

Dq Dq Dε = σki vi,k − hi,i + ρ = σki Dik − hi,i + ρ Dt Dt Dt

(4.34)

This is the local form of the ﬁrst law of thermodynamics for a continuous medium. Note that no kinetic energy term appears in the local form of the ﬁrst law, since it gets canceled out by the rate of work done. Some remarks are in order. The conservation laws derived in this section apply to all materials whether they are ﬂuid or solid, dissipative or elastic (conservative). In particular, the ﬁrst law as derived applies to all materials as well as processes reversible or irreversible. The validity of these equations

© 2005 by Chapman & Hall/CRC Press

150

Continuum Mechanics and Plasticity

is subject to the constraint of a one-to-one and onto transformation which excludes: (a) diffusion processes; (b) chemical effects such as reactions and phase changes; (c) electromagnetic phenomena; and (d) polar media, that is, materials with distributed surface and body moments whose deformation requires account of local rotation and higher order deformation gradients. To address these sophisticated behaviors, the equations would have to be modiﬁed. Nevertheless, the equations in this section provide the foundations for further studies.

4.4

The Constitutive Laws in the Material Description

The local form of conservation laws of Section 4.3 is written based on an inﬁnitesimal material element at the deformed conﬁguration. In particular, the forces are applied to the element at the deformed conﬁguration. In the study of continuum mechanics undergoing large deformation, it is necessary to distinguish between quantities that have been deﬁned with reference to the deformed conﬁguration and those that have been deﬁned with reference to the reference conﬁguration. The former is used in the spatial description of the conservation laws and the latter the material description. It is preferable by some investigators to use one description for solving certain problems and use the other description for other types of problems. The decision is based on the material properties and boundary conditions of the problems. We like to emphasize that, in the material description of conservation laws, the forces are still applied to the element at the deformed conﬁguration, but some quantities as deﬁned are referred to the reference conﬁguration. In this section, we discuss the material description of the constitutive laws.

4.4.1

The Conservation of Mass

The conservation of mass is expressed as dm = ρ0 dV0 = ρ dV

(4.35)

which, from (3.82), may also be written as ρ0 dV = det(F) = J = dV0 ρ

(4.36)

ρ0 = ρ det(F)

(4.37)

or

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

151

This is a form of the conservation of mass and it may also be written as D (ρ det F) = 0 Dt

4.4.2

(4.38)

The Conservation of Momentum

We ﬁrst discuss different stress measures referred to either deformed or undeformed conﬁgurations and then express the conservation of momentum using these stress measures. 4.4.2.1 The Piola–Kirchhoff stress tensors The stress tensor σij that we have been using so far is called the Cauchy stress and it is deﬁned based on a deformed element using the spatial description. The components of σ refer to a Cartesian coordinate system. Sometimes it is desirable to deﬁne stress measures that refer to the undeformed or reference conﬁguration. In this section, we discuss two such stress measures known as the ﬁrst and second Piola–Kirchhoff stresses (or the 1st P–K and 2nd P–K stresses for short). In the instantaneous state (at time t), the inﬁnitesimal force dPi transmitted in the surface element dai is given by (n)

dpi = ti

da = σji nj da = σji daj

or

dp = σT · n da

(4.39)

(0)

For the same inﬁnitesimal force, we may deﬁne a stress vector ti and a stress (0) tensor TRi as in the following expressions. Both new stress vector and stress tensor refer to the initial state. Thus, (0)

(0)

(0)

dpi = ti dA = TRi NR dA = TRi dAR

or (n)

dp = (T(0) )T · N dA

(4.40)

(0)

By comparing (4.39) and (4.40), we see that ti and ti act in the same direction (0) but are different in magnitude. TRi is called the Lagrangian stress, or the 1st P–K stress, and it is also known as the nominal stress. By use of the Nanson’s formula (3.92), we may combine (4.39) and (4.40) to obtain dpi = σji daj = σji J

∂XR (0) dAR = TRi dAR ∂xj

(4.41)

From the last two expressions of (4.41), we ﬁnd the relation between T(0) and σ as (0)

TRi = Jσji

© 2005 by Chapman & Hall/CRC Press

∂XR ∂xj

or

T(0) = JF−1 · σ

(4.42)

152

Continuum Mechanics and Plasticity ti(0)

(0) T13

ti(n) ni (0)

da (0) T11

T12

dA 3 NR(1, 0, 0) 2 1 FIGURE 4.2 First P–K stresses.

With the help of tensor bases, (4.42) may be written as (0)

∂XR eR ⊗ ei · (σmn em ⊗ en ) ∂xi ∂XR ∂XR σmn (eR ⊗ ei ) · (em ⊗ en ) = J =J σmn (ei · em ) · (eR ⊗ en ) ∂xi ∂xi ∂XR ∂XR σin eR ⊗ en = Jσji eR ⊗ e i (4.43) =J ∂xi ∂xj

TRi eR ⊗ ei = J

The components of (4.43) lead to the ﬁrst expression of (4.42). It is useful (0) at this point to illustrate the physical signiﬁcance of the components TRi of the 1st P–K stress. Consider area element dA with a normal NR = [1, 0, 0]. (n) This area is deformed into da with a normal ni . The stress vectors ti and (0) ti for this case are shown in Figure 4.2. They have the same direction but dif(0) ferent magnitudes. The stress vector ti is then decomposed into components (0) (0) (0) T11 , T12 , and T13 with respect to the xi coordinate system. Using a similar (0) procedure, we can consider an area with normal NR [0, 1, 0] to deﬁne T21 , (0) (0) (0) (0) (0) T22 , and T23 ; and a similar approach is used to deﬁne T31 , T32 , and T33 . (0) (0) Note that σij is symmetric, but, from (4.42), TRi is not. Since TRi is not symmetric, this tensor is difﬁcult to use in constitutive equations that are to represent the stress components in terms of the components of the symmetric strain tensor. This difﬁculty can be avoided by deﬁning a symmetric stress called the Piola–Kirchhoff stress (or the 2nd P–K stress), which is now explained. Before the inﬁnitesimal force dpj transmitted in the deformed conﬁguration is referred to the surface element in the reference conﬁguration, let it be subjected to the same transformation that changes the deformed side dxi of the surface element da into the corresponding initial side dXR of dA. That is, we

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

153

~ dp R dpi

NR

dAR XR

dai

ni

xi

V

V0

Rt

R0 FIGURE 4.3 The ﬁctitious force d˜pR .

introduce a ﬁctitious force (or the pseudo-force) d˜pR such that d˜pR =

∂XR dpj ∂xj

(4.44)

which follows the same transformation as in dXR =

∂XR dxj ∂xj

(4.45)

In this operation, the external loading is transformed back to the material description ﬁrst, and the 2nd P–K stress is then deﬁned per unit undeformed area. The ﬁctitious force d˜pR and the initial area dAR have been stretched and rotated the same amount relative to the ﬁnal position dpi and dai , respectively. This deﬁnition of d˜pR is illustrated in Figure 4.3. Using this ﬁctitious force we now deﬁne the 2nd P–K stress tensor RS which refers to the initial area dAR and the relation is d˜pR = SR NS dA = SR dAS

or

dp˜ = · N dA

(4.46)

Note that the form of (4.46) is similar to that of (4.40). We now proceed to determine the relation between RS and σij . Substituting (4.39) into (4.44), we have d˜pR =

∂XR ∂XR ∂XS σkj dak = σkj J dAS ∂xj ∂xj ∂xk

(4.47)

Comparing (4.46) and (4.47), we obtain

RS = Jσjk

© 2005 by Chapman & Hall/CRC Press

∂XR ∂XS ∂xj ∂xk

or

(0) ∂XS

RS = TRi

∂xi

(4.48)

154

Continuum Mechanics and Plasticity

It is then easy to show that (0)

TRi = RS

∂xi ∂XS

(4.49)

(0)

which is the relation between TRi and RS . In the symbolic notation, the above relations may be written as = JF−1 · σ · F−T

and

= T(0) · F−T

where F−T = (F−1 )T

(4.50)

Using the tensor bases, the 2nd P–K stress is written as = RS eR ⊗ eS

(4.51)

Various stress measures are further discussed in Chapter 11 referring to curvilinear coordinates. For the problem of simple shearing, if the XR and the xi systems coincide, that is, the 1-axis is horizontal and the 2-axis vertical, discuss the (0) (0) directions of TRi and ﬁnd the equations relating TRi to the Cauchy stress σij (0) (note that both σij and TRi are Cartesian components). EXAMPLE 4.2

Solution Figure 4.4 shows that a square element is deformed into a parallelogram by simple shearing. The initial areas for Face 1 and Face 2 of the square element are dA(1) and dA(2) and they are deformed into da(1) and da(2) , respectively. (1) (2) The unit normal to the areas are NR and NR and they are deformed into (1) (2) ni and ni , respectively. We now consider the forces and stress components acting on the two faces of the element. (1)

(1)

On face 1: The unit normals are NR = [1, 0] and ni = [cos γ , − sin γ ], where γ is the shearing angle of the element shown in Figure 4.4. The initial and deformed areas are related by da(1) cos γ = dA(1)

(a)

Using (4.39), the inﬁnitesimal force acting on this face is (1)

dpi

(n)1

= ti

(1)

(1)

(1)

da(1) = σji nj da(1) = (σ1i n1 + σ2i n2 ) da(1)

(b)

On the other hand, the same force may be expressed in terms of (4.40) as (1)

dpi

(0)1

= ti

© 2005 by Chapman & Hall/CRC Press

(0)

(1)

(0)

dA(1) = TRi NR dA(1) = T1i dA(1)

(c)

Conservation Laws and Constitutive Equation

155

NR(2) ti(0)2

(0)

T22

(0)

ni(2)

ti(0)1

T21

dA(2)

(0)

T12

ti(n)2

NR(1)

(0)

T11

22

(1)

21

dA

da(2) 2

ti(n)1

12

11

1

ni(1)

da(1)

FIGURE 4.4 Stress components in simple shearing.

By comparing (b) and (c), we obtain (1)

(1)

(0)

(σ1i n1 + σ2i n2 ) da(1) = T1i dA(1)

(d)

which, by use of (a), may be simpliﬁed to yield (0)

σ1i cos γ + σ2i (− sin γ ) = T1i cos γ

(e)

From (e), we obtain (0)

T11 = σ11 − σ21 tan γ

and

(0)

T12 = σ12 − σ22 tan γ

(2)

(f)

(2)

On face 2: The unit normals are NR = [0, 1] and nR = [0, 1], and the area does not change, so that da(2) = dA(2) . Following the same procedure as in Face 1, we ﬁnd (2)

(n)2

= ti

dpi (2)

dpi

(0)2

= ti

(2)

(2)

da(2) = σji nj da(2) = σ2i n2 da(2) = σ2i da(2) (0)

(2)

(0)

(2)

(0)

dA(2) = TRi NR dA(2) = T2i N2 dA(2) = T2i dA(2)

(g) (h)

From (g) and (h), we obtain (0)

(0)

σ2i da(2) = T2i dA(2) = T2i da(2)

with dA(2) = da(2)

(i)

Therefore, we ﬁnd (0)

σ2i = T2i , © 2005 by Chapman & Hall/CRC Press

(0)

σ21 = T21 ,

(0)

σ22 = T22

(j)

156

Continuum Mechanics and Plasticity

We now summarize the stress components found from (f ) and (j) as (0)

(0)

T11 = σ11 − σ21 tan γ , (0)

T21 = σ21 = σ12

and

T22 = σ22 , (0)

(0)

T12 = σ12 − σ22 tan γ

(0)

T12 = T21

(k)

We remark that on Face 1, the normal n(1) is not in the direction of any xi axis. The stress vector t(n)1 is further related to vectors ti , by use of (2.6), acting on cross-sections of the material element that are parallel to the coordinate planes of the xi system, and the vectors ti further deﬁne the components of the Cauchy stress. On the other hand, since N(1) is in the direction of X1 , t(0)1 is already acting on a plane parallel to a coordinate plane, and, therefore, its (0) components with respect to the xi system deﬁne the TRi stress. EXAMPLE 4.3

Find the stress components of Example 4.2 using (4.42).

Solution From (3.20), the simple shear may be described by x1 = X1 + X2 tan γ ,

x2 = X2

(a)

with J = |F| = 1

(b)

The deformation gradient is

1 tan γ 0 1

[F] =

From (4.42), we write σij = J −1

∂xi (0) (0) T = FiR TRj ∂XR Rj

(c)

The components are (0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

σ11 = F1R TR1 = F11 T11 + F12 T21 = T11 + T21 tan γ σ12 = F1R TR2 = F11 T12 + F12 T22 = T12 + T22 tan γ (0)

(0)

(0)

(0)

(0)

(0)

(0)

(0)

σ21 = F2R TR1 = F21 T11 + F22 T21 = T21 σ22 = F2R TR2 = F21 T12 + F22 T22 = T22

These results are the same as those obtained in Example 4.2.

© 2005 by Chapman & Hall/CRC Press

(d) (e) (f) (g)

Conservation Laws and Constitutive Equation

157

For the problem of simple shearing discussed in Example 4.2, ﬁnd the components of the 2nd P–K stress RS .

EXAMPLE 4.4

Solution Using the expression for F found in Example 4.3 and noting that J = |F| = 1, we ﬁnd −1

[F]

∂XS 1 = = 0 ∂xk

− tan γ 1

(a)

From (4.50) we have (0) ∂XS

RS = TRi

(b)

∂xi

Using (a), (b) reduces to (0) (0) T11 − T12 tan γ [ ] = (0) (0) T21 − T22 tan γ

(0)

T12

(0) T22

(c)

Using (k) of Example 4.2, we obtain from (c) (0)

(0)

11 = T11 − T12 tan γ = σ11 − 2σ12 tan γ + σ22 tan2 γ (0)

12 = T12 = σ12 − σ22 tan γ (0)

(d)

(0)

21 = T21 − T22 tan γ = σ12 − σ22 tan γ = 12 (0)

22 = T22 = σ22 In the case of uniform extension along the 1-direction, the applied tensile force is P, shown in Figure 4.5(a); the initial dimensions of the rectangular bar are X1 × X2 × X3 with cross-sectional area A; and the current dimensions are x1 × x2 × x3 with cross-sectional area a. Find the components of σ, T(0) , and . EXAMPLE 4.5

Solution Consider the deformation x1 = λ1 X1 ,

© 2005 by Chapman & Hall/CRC Press

x2 = λ2 X2 ,

x3 = λ3 X3

(a)

158

Continuum Mechanics and Plasticity (a)

2

P

P

(b)

1

2 P

1

P FIGURE 4.5 Effect of rotation on stress components.

The deformation gradient is

λ1 [F] = 0 0

0 λ2 0

0 0 λ3

1 λ1 −1 [F ] = 0 0

0 1 λ2 0

0

0 1 λ3

(b)

and J = det F = λ1 λ2 λ3 . The components of the Cauchy stress are σ11 =

P , a

other components = 0

(c)

The components of the 1st P–K stress may be found from (4.42) in the matrix form as [T (0) ] = J[F−1 ][σ ]

© 2005 by Chapman & Hall/CRC Press

(d)

Conservation Laws and Constitutive Equation

159

and the components of the 2nd P–K stress may be found from (4.50) in the matrix form as [ ] = J[F−1 ][σ ][F−T ]

(e)

Substituting the above information into (d) and (e) and performing the matrix multiplications, we obtain σ

11

λ1 (0) TRi = (λ1 λ2 λ3 ) 0 0

σ

0 0 0

0

, 0 0

RS = (λ1 λ2 λ3 )

11 λ21

0

0 0

0 0

0

0 0

(f)

The nonzero term of T (0) is (0)

T11 = λ2 λ3 σ11 =

x2 x3 a a σ11 = σ11 = X2 X3 A A

P P = a A

(0)

It is seen that T11 is the nominal stress, that is, force over initial area, but σ11 is the true stress. This physical interpretation of T(0) is good only for deformation that does not involve rotation. In the case of simple shear, as discussed in Example 4.2, no such assertion can be made about the 1st P–K stress. The nonzero component of RS is

11 = (λ1 λ2 λ3 )

σ11 λ21

=

λ2 λ3 a σ11 aP 1 1 σ11 = = = λ1 A λ1 A a λ1 λ1

P A

(g)

We see from (g) that no clear physical meaning can be associated with 11 . However, from (4.44), the ﬁctitious force is

1 λ1 −1 [d˜p] = [F ][dp] = 0 0

0 1 λ2 0

0 P P λ1 0 0 =0 0 1 0

(h)

λ3

Thus, (g) may be written as

11 =

d˜p11 A

(i)

It is the component of the ﬁctitious force [d˜p] in the X1 direction divided by the initial cross-sectional area A.

© 2005 by Chapman & Hall/CRC Press

160

Continuum Mechanics and Plasticity

EXAMPLE 4.6 Referring to Example 4.5 and Figure 4.5(b), if, after the stretch, the specimen is rotated 90◦ counterclockwise and the traction P also rotates with it, determine the expressions for the Cauchy stress, the 1st P–K stress, and the 2nd P–K stress components after rotation and thereafter discuss the physical meaning of the three stress tensors.

Solution Let us call the initial stretching of the specimen discussed in Example 4.5 stage 1, and the quantities of this stage are denoted by

λ1 [F(1) ] = 0 0

0 0 λ3

0 λ2 0

σ

0 0

11 λ21

0

0

0 0

0 0

λ1 [T 0(1) ] = (λ1 λ2 λ3 ) 0 0 σ

0

0

0 0 0

P A = 0 0 0 0

11

[ (1) ] = (λ1 λ2 λ3 )

P a [σ (1) ] = 0 0

0 0 0 0 0 0

0 0 0

P Aλ1 = 0 0 0 0

(a)

0

0 0 0 0 0

We now apply a rotation Q to various tensors to obtain the quantities of the second stage denoted by F(2) = Q · F(1) ,

σ(2) = Q · σ(1) · QT

T0(2) = J[F(2) ]−1 · σ(2) = J[F(1) ]−1 · Q−1 · Q · σ(1) · QT = J[F(1) ]−1 · σ(1) = T0(1) · QT (2) = T0(2) · [F(2) ]−T = T0(1) · QT · [[F(1) ]−1 · Q−1 ]T = T0(1) · QT · [Q−1 ]T · [F(1) ]−T = T0(1) · [Q−1 · Q]T · [F(1) ]−T = T0(1) · [F(1) ]−T = (1)

(b)

It is seen from (b) that under a rotation Q, the Cauchy stress σ transforms like a second-rank tensor; the 1st P–K stress transforms like a ﬁrst-rank tensor; and the 2nd P–K stress transforms like a tensor of rank zero.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

161

For this example, the rotation is

0 [Q] = 1 0

−1 0 0

0 0 1

(c)

Using (c) in (b), the stresses in stage 2 are [σ (2) ] = [Q][σ (1) ][Q]T

0 −1 = 1 0 0 0

P 0 a 0 0 1 0

0 0 0

0 0 −1 0 0 0

0

1 0 0 0 = 0 0 1 0

0 0 1 0 0 −1 0 0 = 0 0 0 0 0 1 0 0 0 P 0 0 Aλ1 [ (2) ] = [ (1) ] = 0 0 0 0 0 0

P A [T 0(2) ] = [T 0(1) ][Q]T = 0 0

0

0 P a 0

0 0 0

P A 0 0

0 0 0

(d)

(e)

(f)

We see from (d) that the Cauchy stress has a nonzero component in (2)

σ22 =

P a

(g)

which still lives up to the interpretation of true stress even after the rotation. From (e), we see that the 1st P–K stress has only one nonzero component in 0(2)

T12 =

P , A

0(2)

other TRi = 0

(h)

The second subscript i = 2 indicates that the force P is in the 2-direction, while the ﬁrst subscript R = 1 indicates that this 1st P–K stress component lies on an undeformed area with normal N = [1, 0, 0]. This nonzero component is, therefore, a shear stress and it indicates that the interpretation of nominal stress is no longer appropriate, since a normal stress turns into a shear stress due to rotation. We see from (f) that the 2nd P–K stress does not change due to the imposed rotation. A normal stress before rotation remains a normal stress and a shear stress before rotation remains a shear stress. It is useful from computational viewpoint to deﬁne the 2nd P–K stress, because it is symmetric, it does not change due to imposed rotation, and it is the energy conjugate of Lagrangian

© 2005 by Chapman & Hall/CRC Press

162

Continuum Mechanics and Plasticity

strain E (the concept of work conjugate will be discussed in Section 4.4.3). We note, however, that the physical meaning of the 2nd P–K stress is not clear. In equation (i) of Example 4.5, the 11 component of this stress is the ﬁctitious force divided by initial area A. The ﬁctitious force d˜pR involves stretching and rotation of dpi and, therefore, the 2nd P–K stress does not have the physical meaning of a pure stress. For this reason the 2nd P–K stress should not be used to deﬁne the yield criterion, the fracture criterion, or to set up material instability conditions. 4.4.2.2 Conservation of momentum From (4.39) and (4.40) we have (n)

ti

(0)

da = σji nj da = TRi NR dA

(4.52)

Integrating (4.52) over the surface of the body, we write

S

σij ni da =

S0

(0)

TRi NR dA =

(0)

∂TRi dV0 ∂XR

V0

(4.53)

Let Bi be the body force per unit volume of the undeformed body, we then write Bi dV0 = bi dV

or

Bi = bi

dV = bi J dV0

(4.54)

Integrating (4.54) over the undeformed volume of the body, the resulting total body force is V0

Bi dV0

(4.55)

We note that in the above equations, the forces are applied to the deformed body, although the integrals are over the undeformed body V0 . The momentum is also referred to the deformed body V at time t, and the rate of change of linear momentum is D Dt

V

ρvi dV =

D Dt

V0

ρ0 vi dV0 =

V0

ρ0

Dvi dV0 Dt

(4.56)

Using (4.53), (4.55) and (4.56), the conservation of linear momentum is now

Dvi ρ0 dV0 = Dt V0

© 2005 by Chapman & Hall/CRC Press

V0

(0)

∂TRi dV0 + ∂XR

V0

Bi dV0

(4.57)

Conservation Laws and Constitutive Equation

163

which leads to the following equation of motion in the material description (0)

∂TRi Dvi + Bi = ρ0 ∂XR Dt

(4.58)

In terms of the 2nd P–K stress, the equation of motion becomes ∂ ∂XR

4.4.3

∂xi

RS ∂XS

+ Bi = ρ0

Dvi Dt

(4.59)

The Conservation of Energy

The spatial description for the conservation of energy is given in (4.31). Referring to the undeformed state, this equation can be written as D Dt

1 D ρ0 vi vi dV0 Dt V0 V0 2 D (0) = Bi vi dV0 + TRi NR vi dS0 − hR NR dS0 + ρ0 q dV0 Dt V0 V0 S0 S0 ρ0 ε dV0 +

(4.60) where hR is the component of the heat ﬂux vector referring to the material coordinates, so that hR = (∂XR /∂xi )hi . The energy balance equation (4.60) further becomes Dε Dvi ρ0 ρ0 vi dV0 + dV0 Dt Dt V0 V0 (0) ∂TRi (0) ∂vi vi dV0 = Bi vi dV0 + + TRi ∂XR ∂XR V0 V0 ∂hR Dq − dV0 + ρ0 (4.61) dV0 Dt V0 ∂XR V0 Three terms in the above equation cancel out due to the equation of motion (4.58). We then obtain V0

Dε Dq ∂hR (0) ∂vi ρ0 − TRi dV0 = 0 + − ρ0 Dt ∂XR ∂XR Dt

(4.62)

which leads to the conservation of energy in the local form as ρ0

© 2005 by Chapman & Hall/CRC Press

Dε Dq ∂hR (0) ∂vi = TRi − + ρ0 Dt ∂XR ∂XR Dt

(4.63)

164

Continuum Mechanics and Plasticity

The rate of work term on the right-hand side of (4.63) should be discussed further. This term represents part of work rate that affects the strain energy of a material element (the idea of strain energy is discussed in the later sections of this chapter). This term is sometimes called the speciﬁc rate of work per ˙ is obtained unit mass or the stress power. In this term, the rate of work w using the 1st P–K stress, which may be expressed in terms of the 2nd P–K stress using (4.49). Thus, (0)

TRi

(0)

TRi

∂vi (0) ∂ = TRi ∂XR ∂XR

Dxi Dt

(0)

= TRi

D Dt

∂xi ∂XR

(0) DFiR

= TRi

Dt

(4.64)

∂vi ∂xi ∂vi ∂xi ∂vi ∂xr = RS = RS ∂XR ∂XS ∂XR ∂XS ∂xr ∂XR 1 ∂vi ∂xi ∂xr ∂xi ∂xr DERS ∂vr

RS = RS = + = RS Dir 2 ∂xr ∂xi ∂XS ∂XR ∂XS ∂XR Dt (4.65)

˙ may Equation (3.200) was used in the last expression of (4.65). In addition, w also be expressed in terms of the Cauchy stress. Using (4.42), we write (0)

TRi

∂vi ρ0 ∂XR ∂vi ρ0 ∂vi ρ0 = σji = σji = σji Dij ∂XR ρ ∂xj ∂XR ρ ∂xj ρ

(4.66)

We conclude from (4.64 to 4.66) that the speciﬁc rate of work per unit mass may be written as ˙ = w

1 1 (0) DFiR 1 DERS σij Dij = TRi = RS ρ ρ0 Dt ρ0 Dt

(4.67)

We have thus found three pairs of work (or energy) conjugates. They are σ and D, T(0) and F, and and E. The conjugate stress and strain should be used in any formulation of continuum mechanics problems. Using (4.67), the energy balance equation can also be written as ρ0

4.5

Dε DERS Dq ∂hR + ρ0 = RS − Dt Dt ∂XR Dt

(4.68)

Objective Tensors

Only objective tensors are used to formulate the constitutive equations. Objectivity is also known as reference frame indifference. Tensor quantities that depend only on the orientation of the spatial reference frame, which is given by Q, and not on the other aspects of the motion of the reference frame

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

165

(e.g., translation, velocity and acceleration, angular velocity and angular acceleration) are said to be indifferent, or objective. Consider two observers each having his/her own reference frame. Components of a tensor observed by two different observers are different. This difference is due to the different orientations of the observers but not to relative motions between the observers. In this contest, we are not talking about the change of coordinate system (each observer is free to choose a coordinate system), but are concerned with the change of observer positions and orientations, or the change of reference frame. Therefore, in the discussion of objectivity, transformation of coordinate system does not play any part. The reference frame of an observer may be conveniently denoted by (o, x), where x is a spatial coordinate system with origin O. We may imagine that one observer is attached to the continuous body and moves with the body and the other observer is stationary. Then, the two reference frames attached to the two observers are differed by a translation of the origin and a rotation of orientation. In the general case, both observers may not be stationary. Let us introduce two reference frames (o, x) and (o, ¯ x¯ ) as shown in Figure 4.6. Consider a particle P in the body. The position vector of the particle in (o, ¯ x¯ ) at time t is x¯ and that of the same particle in (o, x) at time t is x. The latter vector is seen by an observer sitting in (o, ¯ x¯ ) as QT · x. These position vectors are thus related by x¯ = c(t) + QT · x

x¯ i = ci + Qji xj

or

(4.69)

where c is the position vector of o in (o, ¯ x¯ ) and Q is an orthogonal tensor that gives the orientation of (o, x) relative to (o, ¯ x¯ ). Thus, (o, x) is different from (o, ¯ x¯ ) by a rigid-body translation c and a rotation Q. Deﬁniton of objective tensors A scalar f , a vector v, and a second-rank tensor T are objective, if for reference frames (o, ¯ x¯ ) and (o, x), related by (4.69), the corresponding scalar f¯, vector v, ¯

P

–

3

3

QT. x

x– o– –

1 FIGURE 4.6 Rotation of reference frames.

© 2005 by Chapman & Hall/CRC Press

o

c –

2

R

1

2

166

Continuum Mechanics and Plasticity

and tensor T¯ are related by f¯ = f

(scalar)

v¯ = QT · v

or

v¯ i = Qji vj

T¯ = QT · T · Q

or

T¯ ij = Qri Qsj Trs

(4.70) (vector) (tensor)

(4.71) (4.72)

We note that a rotation of the body is equivalent to the rotation of the reference frame of the same magnitude but in opposite direction (see Section 1.6). Therefore, if we consider a rigid rotation of the body with ﬁxed reference frame, then (4.69) to (4.72) become x¯ = c(t) + Q · x f¯ = f v¯ = Q · v

(scalar) (vector)

T¯ = Q · T · QT

(tensor)

(4.73) (4.74) (4.75) (4.76)

Either (4.69)–(4.72) or (4.73)–(4.76) may be used to deﬁne objectivity. Since the objectivity should be valid for any rotation Q, we shall make no effort to specify the sense of rotation, when the objectivity of a quantity is being investigated.

4.6

Property of Deformation and Motion Tensors Under Reference Frame Transformation

We investigate the transformation property of tensors F, C, B, v, L, D, and W. Using (4.69), the transformation equation for FiR is ∂ x¯ i ∂ x¯ i ∂xk ∂xk = = Qki (t) = Qki FkR F¯ iR = ∂XR ∂xk ∂XR ∂XR

(4.77)

which may be written in the matrix form as ¯ = [Q]T [F] [F]

(4.78)

that is, F behaves like a vector in a rotation QT of the body or a rotation Q of the spatial reference frame. Note that since Q is arbitrary, we can use either Q or QT in the discussion of objectivity. Even though F is a second-rank tensor, it transforms as a vector in the reference frame transformation (also referred to as the observer transformation). This rule of transformation should be expected, because only subscript i in FiR refers to the spatial reference frame.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

167

In the case of C, the expression is ∂xk ∂xn ∂xk ∂xn ∂ x¯ m ∂ x¯ m C¯ RS = = Qkm Qnm = Qkm Qnm ∂XR ∂XS ∂XR ∂XS ∂XR ∂XS ∂xk ∂xn ∂xk ∂xk = δkn = = CRS ∂XR ∂XS ∂XR ∂XS

(4.79)

Thus, C transforms like a scalar in the observer transformation. The left Cauchy–Green deformation tensor B transforms like ∂ x¯ i ∂ x¯ j ∂xk ∂xm B¯ ij = = Qki Qmj = Qki Qmj Bkm ∂XR ∂XR ∂XR ∂XR

(4.80)

which may be written in the matrix form as ¯ = [Q]T [B][Q] [B]

(4.81)

Thus, B transforms like a second-order tensor in the observer transformation. Consider now the observer transformation of velocity vi . Differentiating (4.69), we have D¯xi ˙ ji xj = v¯ i = Qji vj + Q Dt

(4.82)

Inverting the relation (4.69) and letting ci = 0, (4.82) becomes ˙ ji Qjk x¯ k v¯ i = Qji vj + Q

(4.83)

We see from (4.83) that vi is a ﬁrst-rank tensor, but under the observer transformation, it is not objective. If it were objective, we would have v¯ i = Qji vj for any Qij . Note that in the rigid rotation of the spatial reference frame, the spin of the frame is related to Qij through (3.184), (3.187), and (3.188), and ˙ ij Qkj = ik = ekij ωj . Therefore, given by Q v¯ = QT · v + ω × r

(4.84)

The velocity gradient is now investigated by differentiating (4.83). We obtain v¯ i,r =

∂vj ∂xs ∂ v¯ i ˙ ji Qjr = Qji Qsr vj,s + Q ˙ ji Qjr = Qji +Q ∂ x¯ r ∂xs ∂ x¯ r

(4.85)

This shows that the velocity gradient tensor is not an objective tensor either because of the presence of the second term on the right-hand side of (4.85).

© 2005 by Chapman & Hall/CRC Press

168

Continuum Mechanics and Plasticity

We show that the symmetric part of vi,j is objective, whereas the antisymmetric part of vi,j is not. To this end, we interchange i and r to obtain ∂ v¯ r ˙ jr Qji = Qjr Qsi vj,s + Q ∂ x¯ i

(4.86)

Adding (4.85) and (4.86), we ﬁnd ¯ ir = 1 D 2

∂ v¯ r ∂ v¯ i + ∂ x¯ r ∂ x¯ i

=

1 1 ˙ ˙ {Qji Qsr vj,s + Qjr Qsi vj,s } + {Q ji Qjr + Qjr Qji } 2 2 (4.87)

We note that since D ˙ ji Qjr + Q ˙ jr Qji = D (δir ) = 0 (Qji Qjr ) = Q Dt Dt

(4.88)

Equation (4.87) becomes ¯ ir = Qji Qsr Djs D

(4.89)

Therefore, Dij is an objective tensor. It is not surprising that Dij is objective, because Dij represents the rate of deformation that describes the rate of stretching of line elements, and this stretching may be measured by a ruler and is independent of the orientation of the observer. Now, let us consider the antisymmetric part of vi,j . From (4.85) and (4.86), we obtain ¯ ir = 1 W 2

∂ v¯ r ∂ v¯ i − ∂ x¯ r ∂ x¯ i

1 ˙ ˙ = Qji Qsr Wjs + (Q ji Qjr − Qjr Qji ) 2

˙ ji Qjr = Qji Qsr Wjs + Q

(4.90)

Because of the presence of the second term, the spin tensor is not objective. ˙ jr Qji = −Q ˙ ji Qjr . In The last expression has been obtained by observing that Q the case of rigid-body motion, Lij = Wij = ij , and (4.90) is reduced to ¯ ir = Qji Qsr js + ir

(4.91)

In the symbolic notation, equations (4.85), (4.89), and (4.90) are written as ˙ T · Q, L¯ = QT · L · Q + Q

(4.92a)

T

¯ = Q · D · Q, D

(4.92b)

˙T·Q ¯ = QT · W · Q + Q W

(4.92c)

It is seen that L and W depend on the spin of the rotating system, but D depends only on the orientation of the reference (spatial) frame. Note that

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

169

for two chosen coordinate systems, L transforms like a second-rank tensor if ˙ = 0. Q

4.7

Objective Rates

In the small strain mechanics, constitutive equations of the rate form have been widely used. Investigators have used the stress, stress rate, and higher-order stress rates on the one hand and the strain, strain-rate, and higher-order strainrates on the other to propose constitutive equations of the following form f (σ , σ˙ , σ¨ , . . .) = g(ε, ε˙ , ε¨ , . . .)

(4.93)

where f and g are nonlinear functions generally. When the mechanics of ﬁnite strain is of interest, we ask the question regarding the appropriate rates to use in the constitutive equations. We emphasize here that only objective tensors and objective rates can be used.

4.7.1

Some Objective Rates

Supposing that a symmetric tensor T is an objective tensor, such that T¯ = QT · T · Q

(4.94)

then, we inquire whether the rate DT/Dt is objective. If this rate is not objective, then we cannot interpret the physical signiﬁcance using it. To answer the above question, we differentiate (4.94) to obtain DT¯ D ˙ T · T · Q + QT · T˙ · Q + QT · T · Q ˙ = (QT · T · Q) = Q Dt Dt

(4.95)

The superposed “dot” denotes the material derivative. The presence of ˙ T · T · Q and QT · T · Q ˙ in (4.95) shows that T˙ is not objective. Q ˙ and Q ˙ T from (4.95), To determine an objective derivative, we eliminate Q since these terms cannot appear in a reference frame transformation. From equation (4.92a), we obtain ˙T L¯ · QT = QT · L · Q · QT + Q

or

˙ T = L¯ · QT − QT · L Q

(4.96)

By taking the transpose of (4.96), we obtain ˙ = Q · L¯ T − LT · Q Q

© 2005 by Chapman & Hall/CRC Press

(4.97)

170

Continuum Mechanics and Plasticity

By substitution, we then have from (4.95) DT¯ = (L¯ · QT − QT · L) · T · Q + QT · T˙ · Q + QT · T · (Q · L¯ T − LT · Q) Dt = L¯ · QT · T · Q − QT · L · T · Q + QT · T˙ · Q + QT · T · Q · L¯ T − QT · T · L T · Q = L¯ · T¯ − QT · L · T · Q + QT · T˙ · Q + T¯ · L¯ T − QT · T · LT · Q

(4.98)

Equation (4.98) can be rearranged into the following form DT¯ − L¯ · T¯ − T¯ · L¯ T = QT · Dt

DT − L · T − T · LT · Q Dt

(4.99)

It follows that the derivative ((DT/Dt)−L·T−T·LT ) is an objective derivative. This derivative may also be expressed in the index notation as DTij − vi,k Tkj − Tik vj,k Dt

(4.100)

Similarly, we can show that the following rates are objective rates. The Jaumann rate is given by T∇ =

DT −W·T+T·W Dt

and

T¯ ∇ = QT · T∇ · Q

(4.101)

and

T¯ ∗ = QT · T∗ · Q

(4.102)

and the convected rate is given by T∗ =

DT + LT · T + T · L Dt

The Jaumann rate deﬁned in (4.101) is based on the spin tensor W. We may use another tensor ω, which represents the rate of rotation of some physical quantity to deﬁne the same objective rate. In this case, (DT/Dt)−ω·T+T·ω is called the co-rotational rate. The physical signiﬁcance and application of these rates will be discussed later in connection with some constitutive models. Finally, we note that, if T is stress, then these are objective stress rates. EXAMPLE 4.7

Derive the convected rate.

Solution We have from (4.92a) ˙ T · Q = QT · L · Q − Q T · Q ˙ L¯ = QT · L · Q + Q

© 2005 by Chapman & Hall/CRC Press

(a)

Conservation Laws and Constitutive Equation

171

Multiplying (a) from the left by Q, we obtain ˙ Q · L¯ = L · Q − Q

˙ = L · Q − Q · L¯ or Q

(b)

Taking the transpose of (b), we have ˙ T = QT · LT − L¯ T · QT Q

(c)

Hence, after substitution of (b) and (c), (4.95) becomes DT¯ ¯ = (QT · LT − L¯ T · QT ) · T · Q + QT · T˙ · Q + QT · T · (L · Q − Q · L) Dt = QT · LT · T · Q − L¯ T · T¯ + QT · T˙ · Q + QT · T · L · Q − T¯ · L¯ = QT · (T˙ + LT · T + T · L) · Q − L¯ T · T¯ − T¯ · L¯

(d)

From (d), we write DT¯ + L¯ T · T¯ + T¯ · L¯ = QT · Dt

DT T +L ·T+T·L ·Q Dt

(e)

which shows that (DT/Dt + LT · T + T · L) is an objective rate. In the index notation, the convected rate is written as DTij + Tim vm,j + Tmj vm,i Dt EXAMPLE 4.8

(f)

Derive the Jaumann rate.

Solution From (4.92), we have ¯ = QT · W · Q + Q ˙ T · Q = QT · W · Q − Q T · Q ˙ W

(a)

Multiplying (a) by Q from the left, we have ¯ =W·Q−Q ˙ Q·W

˙ =W·Q−Q·W ¯ or Q

(b)

Taking the transpose of (b), we obtain ˙ T = QT · WT − W ¯ T · QT Q

© 2005 by Chapman & Hall/CRC Press

(c)

172

Continuum Mechanics and Plasticity

Substituting (b) and (c) into (4.95), we ﬁnd DT¯ ¯ T · QT ) · T · Q + QT · T˙ · Q + QT · T · (W · Q − Q · W) ¯ = (QT · WT − W Dt ¯ T · T¯ + QT · T˙ · Q + QT · T · W · Q − T¯ · W ¯ = QT · W T · T · Q − W ¯ T · T¯ − T¯ · W ¯ = QT · (T˙ + WT · T + T · W) · Q − W

(d)

From (d) we conclude that DT¯ ¯ T · T¯ + T¯ · W ¯ = QT · +W Dt

DT + WT · T + T · W · Q Dt

(e)

DT −W·T+T·W ·Q Dt

(f)

But WT = −W, (e) then becomes DT¯ ¯ · T¯ + T¯ · W ¯ = QT · −W Dt

Therefore, T∇ =

DT −W·T+T·W Dt

(g)

is an objective rate.

4.7.2

Physical Meaning of the Jaumann Stress Rate

Let a body spin with an angular velocity w with reference frame at time t denoted by xi . Let x¯ i be another reference frame which is attached to the body and spins with it. Let x¯ i coincide with xi at time t, when the stress at a generic point P in the body is σ¯ ij (t) = σij (t). At time t + dt, the stress at particle P is σ¯ ij (t + dt) referred to the rotating axes x¯ i . Then, according to Jaumann, the stress rate may be deﬁned as 1 [σ¯ ij (t + t) − σ¯ ij (t)] t→0 t

σij∇ = lim

(4.103)

The relation Qij between the two reference frames may be found by considering the spin of the reference frame (see Figure 4.7) which rotates base vectors ei into e¯ i . From (1.22), the relation is e¯ i = Qji ej

© 2005 by Chapman & Hall/CRC Press

(4.104)

Conservation Laws and Constitutive Equation

173

–

ei dt

dei

ei FIGURE 4.7 Spin of the reference frame.

The angle of rotation is ω dt, where ω is the angular velocity. Using n to denote the unit normal to the plane formed by ei and e¯ i , the angular velocity vector is w = ωn = ωni ei = wi ei

(4.105)

Therefore, wi = ωni . Referring to Figure 4.7, we write e¯ i = ei + dei = ei + w dt × ei

(4.106)

Using (4.104), (4.106) becomes Qji ej = ei + ωnj dtej × ei = ei + ωnk dt eijk ej

(4.107)

The components of (4.107) are Qji = δij + ωnk dteijk

(4.108)

Qij = δij − ωnk dteijk

(4.109)

which may be rewritten as

Equation (4.109) describes the rotation of the reference frame. This equation may be compared with (1.118) and the same result can be obtained from (1.118) by setting cos α = 1, sin α = α, α = ω dt, and wk = ωnk . The stress tensor at P at time t + dt referred to the reference frame xi is

σij (t + dt) = σij (t) +

© 2005 by Chapman & Hall/CRC Press

Dσij dt Dt

(4.110)

174

Continuum Mechanics and Plasticity

The stresses σ¯ ij (t+dt) and σij (t+dt), referring to x¯ i and xi systems, respectively, are related by σ¯ ij = Qpi Qqj σpq , so that by use of (4.109), we write σ¯ ij (t + dt) = Qpi Qqj σpq (t + dt)

Dσpq = (δpi − epim wm dt)(δqj − eqjn wn dt) σpq (t) + dt Dt Dσij = σij (t) + − epim wm σpj − eqjn wn σiq dt + O(dt2 ) Dt (4.111)

Hence, by neglecting the higher order terms in dt and using (4.103), we obtain σij∇ =

Dσij − epim wm σpj − eqjn wn σiq Dt

(4.112)

Noting that Wjk = −eijk wi

and

−Wjq = Wqj

(4.113)

we then have σij∇ =

D σij − Wip σpj + σiq Wqj Dt

(4.114)

This is the Jaumann stress rate and is the same as the expression in (4.101).

4.8

Finite Elasticity

We study the topic of elasticity in the remaining part of this chapter. Elasticity investigates the speciﬁc material behavior which is reversible, that is, if a material is elastic, then upon the removal of loading, the material will recover its original state. Elastic material is an ideal material and it is a good approximation for most materials in the small strain range. In the ﬁnite strain range, rubber is known to exhibit an elastic behavior to a good approximation. There are several approaches to formulating the constitutive equation for an elastic material. The Cauchy elasticity is discussed ﬁrst and then the hyperelasticity. Emphasis is given to hyperelasticity and provide several examples in the application. Finally, in the last section of this chapter, hypo-elasticity is discussed, which, strictly speaking, is not elasticity.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation 4.8.1

175

The Cauchy Elasticity

In the investigation of a constitutive equation, we consider the stress and deformation of an inﬁnitesimal material element. If the material is elastic, then the stress σ is, by deﬁnition, a function of the current deformation written as σ = g(F)

(4.115)

where g is a tensor-valued function of F and is in general a nonlinear function. We use the deformation gradient F to denote deformation for the purpose of generality, and we show next by use of objectivity that the deformation cannot be represented by F. Under observer transformation of (4.69), an arbitrary QT , (4.115) is written in the barred frame as ¯ σ¯ = g(F)

(4.116)

which by use of (4.71) and (4.72) is QT · σ · Q = g(QT · F)

(4.117)

QT · g(F) · Q = g(QT · F)

(4.118)

or

for an arbitrary orthogonal Q. Equation (4.118) gives the restriction on the form of g in (4.115). In particular, if we choose Q = R and, by applying F = R · U from the polar decomposition theorem, we obtain QT · F = RT · F = RT · R · U = U

(4.119)

Note that the observer transformation is valid for any Q, but if we make a special choice of it, we can observe useful information from this orientation of the observer. The information is still there, but it cannot be visualized from another orientation Q. Making use of (4.119), (4.118) becomes RT · g(F) · R = g(U)

(4.120)

Combining (4.115) and (4.120), we obtain σ = R · g(U) · RT

(4.121)

We see from (4.121) that σ depends on a nonlinear function of U and depends on R explicitly. But, since U is related to C from (3.40) and C is related to E from (3.100), equivalent forms of (4.121) are σ = R · f(C) · RT

© 2005 by Chapman & Hall/CRC Press

(4.122)

176

Continuum Mechanics and Plasticity

and σ = R · h(E) · RT

(4.123)

where f is a tensor-valued function of C and h is a tensor-valued function of E. One of (4.121), (4.122), or (4.123) may be used as the constitutive equation for anisotropic elastic materials. For a given deformation, R, U, C, and E can be determined. If explicit functions g, f, or h are known, then by use of one of the above constitutive equations the stress σ may be determined. In the case that the material is isotropic, (4.122) may be rewritten as σˆ ≡ RT · σ · R = f(C)

(4.124)

Following a representation theorem of Rivlin and Ericksen [1] for an isotropic tensor function of a tensor, (4.124) is written as σˆ = ϕ0 1 + ϕ1 C + ϕ2 C2

(4.125)

where ϕ0 , ϕ1 , and ϕ2 are scalar invariant functions of the three principal invariants of C. Equation (4.125) can also be derived by expressing the function f in (4.124) as a polynomial of C and applying the Cayley–Hamilton theorem (Section 2.15) successively. From (2.104), we write C3 = I1 C2 − I2 C + I3 I

(4.126)

where I1 , I2 , and I3 are principal invariants of C. By successive applications of (4.126), (4.124) reduces to (4.125). From (4.125), we have σ = R · σˆ · RT = R · (ϕ0 1 + ϕ1 C + ϕ2 C2 ) · RT = ϕ0 R · RT + ϕ1 R · C · RT + ϕ2 R · C · CT · RT

(4.127)

The last term of (4.127), using (3.37), is R · C · CT · RT = R · C · (RT · R) · CT · RT = (R · C · RT ) · (R · C · RT )T = B · BT (4.128) Substituting (3.37) and (4.128) into (4.127), we obtain σ = ϕ0 1 + ϕ1 B + ϕ2 B2

(4.129)

where ϕk = ϕk (I1 , I2 , I3 ) and we note that the principal invariants of C and B are the same. By use of the Cayley–Hamilton theorem, (4.129) may be written in a slightly different form. From (2.104), we write B3 − I1 B2 + I2 B − I3 1 = 0

© 2005 by Chapman & Hall/CRC Press

(4.130)

Conservation Laws and Constitutive Equation

177

Multiplying (4.130) by B−1 , we get B2 = I1 B − I2 1 + I3 B−1

(4.131)

Finally, we substitute (4.131) into (4.129) to obtain σ = α0 1 + α1 B + α−1 B−1

(4.132)

where α0 = ϕ0 − ϕ2 I2 ,

α1 = ϕ1 + ϕ2 I1 ,

α−1 = ϕ2 I3

(4.133)

Either (4.129) or (4.132) can be used as the constitutive equation for an isotropic elastic material. 4.8.2

Hyperelasticity

A material is called hyperelastic or Green-elastic if there exists an elastic potential function, widely known as the strain-energy density function W , which is a scalar function of one of the strain or deformation tensors. Hyperelasticity uses the conservation of energy principle, leaving out the thermal effect. We postulate that the elastic material is capable of storing strain-energy and write Rate of work done on body R

Rate of change of strain-energy in R

=

(4.134)

It may be shown that the strain-energy density is equal to the Helmholz free energy for isothermal process and is equal to the internal energy for isentropic process. This is further discussed in a later chapter. But, we mention for now that the free energy is the portion of internal energy available for doing work at constant temperature. If the strain-energy density W is deﬁned per unit undeformed volume, then Total strain-energy =

W dV0 =

W

dV0 dV = dV

ρ W dV ρ0

(4.135)

The rate of change of the strain-energy is then D Dt

ρ W dV = ρ0

ρ DW dV ρ0 Dt

(4.136)

and the rate of work done is (n) ti vi dS = σki nk vi dS = (σki vi ),k dV = (σki,k vi + σki vi,k ) dV S

S

V

V

(4.137)

© 2005 by Chapman & Hall/CRC Press

178

Continuum Mechanics and Plasticity

But the term V (σki,k vi )dV in (4.137) cancels out with the kinetic energy term and the body force term by use of the equation of motion as discussed in Section 4.3.3. Therefore, the rate of work done that affects the rate of change of strain-energy is V

σki vi,k dV

(4.138)

Substituting (4.136) and (4.138) into (4.134), this balance of energy in the local form, is given by ρ DW ∂vi ∂XR = σji vi,j = σji ρ0 Dt ∂XR ∂xj

(4.139)

or by use of (4.42) ρ0 ∂XR ∂vi DW (0) ∂vi (0) ∂ = TRi = TRi = σji Dt ρ ∂xj ∂XR ∂XR ∂XR ∂xi (0) D (0) DFiR = TRi = TRi Dt ∂XR Dt

Dxi Dt

(4.140)

(0)

where TRi is the 1st P–K stress. In the case of elastic material, the stress is a function of current deformation. If the deformation is expressed by the deformation gradient FiR , the strainenergy density W is a function of FiR . Thus, DW (FiR ) ∂W DFiR = Dt ∂FiR Dt

(4.141)

By the substitution of (4.141) into (4.140), we then obtain

∂W (0) − TRi ∂FiR

DFiR =0 Dt

(4.142) (0)

Since this equation should hold for all DFiR /Dt and since W and TRi are functions of FiR , but independent of DFiR /Dt, the left-hand side of the above equation must vanish for all arbitrary value of DFiR /Dt. It follows that (0)

TRi =

∂W ∂FiR

(4.143)

or, by use of (4.42), σij =

© 2005 by Chapman & Hall/CRC Press

∂W ρ ∂xi ∂W (F) ρ = FiR ρ0 ∂XR ∂FjR ρ0 ∂FjR

(4.144)

Conservation Laws and Constitutive Equation

179

This is the most general constitutive equation of an elastic material undergoing ﬁnite deformation if we make use of the strain-energy density function. In the last step, the symmetric property of σij is invoked. We now consider the effect of objectivity on the form of strain-energy function W . By applying objectivity, we have in the barred reference frame σij =

¯ ¯ ∂FrS ∂W ρ ¯ ∂W ρ FiR = F¯ iR ρ0 ρ0 ∂FrS ∂ F¯ jR ∂ F¯ jR

(4.145)

But, from (4.78), F¯ iR = Qki FkR ,

FrS = Qrm F¯ mS ,

∂FrS = Qrm δmj δSR = Qrj δSR ∂ F¯ jR

(4.146)

Hence, after substitution, (4.145) becomes σ¯ ij =

¯ ¯ ∂W ρ ∂W ρ Qki FkR Qrj δSR = Qki Qrj FkR ρ0 ∂FrS ρ0 ∂FrR

(4.147)

Therefore, by comparing (4.147) with (4.144), we conclude that σ¯ ij = Qki Qrj σkr

or

σ¯ = QT · σ · Q

¯ (F) ¯ if W (F) = W

(4.148)

which states that objectivity of the stress tensor is satisﬁed if the strain-energy density W is form-invariant with rotation of the spatial reference frame. Hence, ¯ (F) ¯ = W (F) ¯ = W (F) W

(4.149)

The last equality is equivalent to the condition that W (QT · F) = W (F)

for any orthogonal Q

(4.150)

In particular, if we choose Q = R and, by applying F = R · U from the polar decomposition theorem, we obtain QT · F = R T · F = R T · R · U = U

(4.119)

as in the discussion of the Cauchy elasticity. Therefore, by substituting (4.119) into (4.150), we obtain W (F) = W (U)

© 2005 by Chapman & Hall/CRC Press

(4.151)

180

Continuum Mechanics and Plasticity

which means that W depends on F only through its dependence on U. But, since U is related to C by (3.40), the strain-energy density may also be expressed in terms of C as √ ˜ (C) = W (C) W (U) = W ( C) = W

(4.152)

The tilde in the last expression has been dropped for simplicity. We may do this, since the function is as yet unspeciﬁed. We have thus shown from the application of objectivity that the strain-energy density function is a function of the right Cauchy–Green deformation tensor C. Using this property, we now have ∂W ∂W ∂CST ∂W ∂((∂xi /∂XS )(∂xi /∂XT )) = = ∂FjR ∂CST ∂FjR ∂CST ∂(∂xj /∂XR ) ∂W ∂xi ∂xi = δij δSR + δij δTR ∂CST ∂XT ∂XS =

∂W ∂xj ∂W ∂xj ∂W ∂xj + =2 ∂CRT ∂XT ∂CSR ∂XS ∂CSR ∂XS

(4.153)

Note that the last equality is obtained by observing the symmetric property of CRS . Therefore, the stress of equation (4.144) can be written as σij = 2

ρ ∂xi ∂xj ∂W ρ0 ∂XR ∂XS ∂CRS

(4.154)

In terms of the 2nd P–K stress tensor, the constitutive equation for hyperelastic material is given from (4.48) and (4.154) by

RS = Jσjk =2

∂xj ∂xk ∂W ∂XR ∂XS ∂XR ∂XS =2 ∂xj ∂xk ∂XP ∂XQ ∂CPQ ∂xj ∂xk

∂W ∂W δPR δQS = 2 ∂CPQ ∂CRS

(4.155)

Hence,

RS = 2

∂W (C) ∂W (E) = ∂CRS ∂ERS

(4.156)

where ERS is the Lagrangian strain tensor deﬁned by (3.100). It is seen that by use of the 2nd P–K stress, the stress is the partial derivative of the strainenergy density function with respect to a deformation tensor. The constitutive equation is thus greatly simpliﬁed. We note that this equation applies to fully anisotropic elastic materials.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation 4.8.3

181

Isotropic Hyperelastic Materials

A material is said to be isotropic, if its constitutive equation remains forminvariant with rotation of the material coordinate system XR . This statement is similar to that of material objectivity. The difference is that we rotate the material coordinate system here. The isotropic statement imposes a constraint on the constitutive equations (4.154) and (4.156), and, since in hyperelasticity the stress is expressed in terms of the strain-energy density function, the constraint of isotropy is imposed on the strain-energy density W(C). Therefore, we state that an elastic material is isotropic if its strain-energy density function is form-invariant with rotation of the material coordinate system. Anecessary and sufﬁcient condition that W (C) be form-invariant with rotation of the material coordinate system is that W is a function only of the invariants of CRS , and not a function of the components of CRS .

THEOREM

Proof From the spectral representation (2.95) of a symmetric second-rank tensor by its eigenvalues and eigenvectors, we write CRS =

(Q)

(Q)

CQ N R N S

(1)

(1)

(2)

(2)

(3)

(3)

= C1 N R N S + C 2 N R N S + C 3 N R N S

(4.157)

Q

Then, the strain-energy density function is given by (1)

(2)

(3)

W = W (C1 , C2 , C3 ; NR , NR , NR

(4.158) (Q)

where the eigenvalues CQ remain invariant on the rotation of XR ; and NR are the eigenvectors. We now make use of a theorem on invariants (see Green and Adkins [2]) which states that: a scalar-valued function φ(α(1) , α(2) , . . . , α(m) ) of m vectors α(1) , α(2) , . . . , α(m) is invariant under all proper orthogonal transformations if and only if it can be expressed as a function of all possible inner products α(r) · α(s) (r, s = 1, 2, . . . , m) and the determinant |α(r) |, that is, φ = φ(α(r) · α(s) , |α(r) |)

(4.159)

In the case of (4.158), the eigenvectors are orthogonal so that (P)

(Q)

N R NR

= δPQ

and

(P)

|NR | = 1

(4.160)

Therefore, the strain-energy function is W = W (C1 , C2 , C3 )

© 2005 by Chapman & Hall/CRC Press

(4.161)

182

Continuum Mechanics and Plasticity

In the above expression, the indices 1, 2, and 3 are arbitrarily chosen depending on the designation of the coordinate axes. Since W must be a symmetric function of C1 , C2 , and C3 , it must be form-invariant with permutation of the indices, that is, W (C1 , C2 , C3 ) = W (C1 + C2 + C3 , C1 C2 + C2 C3 + C3 C1 , C1 C2 C3 )

(4.162)

or W = W (I1 , I2 , I3 )

(4.163)

where I1 , I2 , and I3 are the three principal invariants of CRS deﬁned in Section 3.6.4 and this concludes the proof of the theorem. To obtain the constitutive equation for isotropic hyperelastic material, we consider ∂W ∂I1 ∂W ∂I2 ∂W ∂I3 ∂W = + + ∂CRS ∂I1 ∂CRS ∂I2 ∂CRS ∂I3 ∂CRS

(4.164)

where ∂I1 = δRS, ∂CRS

∂I2 = I1 δRS − CRS, ∂CRS

∂I3 −1 = cofactor(CRS ) = I3 CRS ∂CRS (4.165)

The expressions for the three invariants are given in Sections 2.12 and 3.6.4. In particular, we mention here that I2 = 12 (I12 − CRS CRS )

(4.166)

By substitution, we then obtain from (4.156)

RS = 2

∂W ∂W ∂I1 ∂W ∂I2 ∂W ∂I3 =2 + + ∂CRS ∂I1 ∂CRS ∂I2 ∂CRS ∂I3 ∂CRS

(4.167)

or

RS = 2

∂W −1 ∂W ∂W δRS + (I1 δRS − CRS ) + I3 C ∂I1 ∂I2 ∂I3 RS

(4.168)

To express the above equation in terms of the Cauchy stress, we obtain from (4.50) σij =

© 2005 by Chapman & Hall/CRC Press

ρ ∂xi ∂xj

RS ρ0 ∂XR ∂XS

(4.169)

Conservation Laws and Constitutive Equation

183

Using (4.168), each term in (4.169) needs to be multiplied by a factor and these terms are ∂xi ∂xj ∂xi ∂xj δRS = = Bij = left Cauchy–Green tensor ∂XR ∂XS ∂XR ∂XR ∂xi ∂xj ∂xi ∂xj CRS = ∂XR ∂XS ∂XR ∂XS

∂xk ∂xk ∂XR ∂XS

=

∂xi ∂xk ∂XR ∂XR

∂xk ∂xj ∂XS ∂XS

(4.170) = Bik Bkj (4.171)

∂xi ∂xj ∂XR ∂XS ∂xi ∂xj −1 C = ∂XR ∂XS RS ∂XR ∂XS ∂xk ∂xk ∂xj ∂XS ∂xi ∂XR = = δik δjk = δij ∂XR ∂xk ∂XS ∂xk

(4.172)

By substituting these expressions into (4.168) and (4.169), we obtain 2 σij = √ I3

∂W ∂W ∂W Bij + (I1 Bij − Bik Bkj ) + I3 δij ∂I1 ∂I2 ∂I3

(4.173)

or 2 σij = √ I3

∂W ∂W + I1 ∂I1 ∂I2

∂W ∂W Bij − Bik Bkj + I3 δij ∂I2 ∂I3

ρ0 2 with I3 = ρ (4.174)

Equation (4.174) is the constitutive equation for isotropic hyperelasticity and we observe that the scalar coefﬁcients of (4.174) are derived from a single scalar function W (I1 , I2 , I3 ). Equation (4.174) has the same form as the constitutive equation (4.129) of Cauchy elasticity. But, in the case of Cauchy elasticity, there are three scalar functions ϕk (I1 , I2 , I3 ) which need to be determined from experiments. We now discuss the constraints due to incompressibility. Under moderate stress 10,000 psi (68.9 MPa), the assumption of incompressibility is valid for rubber. When the material is incompressible, we can write I3 =

ρ0 ρ

2

=1

(4.175)

In this case ∂W /∂I3 |I3 =1 is indeterminate and is no longer a material property. Incompressibility is a kinematic constraint expressed by vi,i = Dii = 0. The mechanical effect of such a constraint is to give rise to an arbitrary hydrostatic pressure −p1 which does no work. From the energy equation (4.34),

© 2005 by Chapman & Hall/CRC Press

184

Continuum Mechanics and Plasticity

the term σki vi,k = σki Dik is not affected by superimposed hydrostatic pressure, that is, (σki − pδki )Dik = σki Dik − pδki Dik = σki Dik − pDii = σki Dik

(4.176)

Incompressible materials are capable only of isochoric deformations. The arbitrary hydrostatic pressure is not given by a constitutive equation but is determined by the equations of motion (or equilibrium) and boundary conditions. In this case, the strain-energy density function is written as W (I1 , I2 ) and from (4.173) the hyperelastic constitutive equation for incompressible material is written as σij = 2{W1 Bij + W2 (I1 Bij − Bik Bkj ) − pδij }

(4.177)

where Wi = ∂W /∂Ii . By use of the Cayley–Hamilton theorem (4.177) may also be written as σij = −pδij + 2W1 Bij − 2W2 B−1 ij

(4.178)

EXAMPLE 4.9 The hydrostatic pressure is expressed in the form of Cauchy stress by σij = −pδij . Find corresponding expressions using the 1st and 2nd P–K stresses and discuss the physical meanings of these expressions, if any. Consider cases where the deformation gradient F has or does not have a diagonal form.

Solution From (4.42) and (4.48), we have ∂XR ∂XR = −Jp ∂xj ∂xi

(a)

∂XR ∂XS ∂XR ∂XS −1 = −Jp = −JpCRS ∂xj ∂xk ∂xk ∂xk

(b)

(0)

TRi = −Jpδji

RS = −Jpδjk

If F has a diagonal form such as

λ1 [F] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 λ2 0

0 0 λ3

1 λ1 −1 [F ] = 0 0

0 1 λ2 0

0

0 1 λ3

(c)

Conservation Laws and Constitutive Equation

185

then (a) and (b) become

(0)

TRi

1 λ1 = −Jp 0 0

0 1 λ2 0

0

0 1 λ3

RS

1 λ2 1 = −Jp 0 0

0

0

1 λ22 0

0 1

(d)

λ23

There are only normal components in both stress tensors and the sum of the diagonal terms for both cases are

tr T

(0)

1 1 1 = −Jp + + λ1 λ2 λ3

tr = −Jp

1 λ21

+

1 λ22

+

1 λ23

(e)

We see from (e) that both tr T(0) and tr are multiples of the hydrostatic stress p, but affected by the stretching or contraction of the material element through λi . (0) If F does not have the diagonal form, then both TRi and RS do not have the diagonal form. In other words, even though we can still ﬁnd tr T(0) and tr and both are multiples of the hydrostatic stress p, shear stresses arise in (0) both TRi and RS so that it is fair to say that the 1st and 2nd P–K stresses are hydrostatic pressure sensitive, while the Cauchy stress is not. The shear components of the Cauchy stress are not affected by the superimposed hydrostatic pressure.

4.8.4

Applications of Isotropic Hyperelasticity

This section discusses some simple applications of the constitutive equation for isotropic hyperelasticity. If the strain-energy function W is known for an incompressible material, then the stress is determined by (4.177) or (4.178) up to a hydrostatic pressure, which is in turn determined from the boundary condition. The complexity of the governing equations usually calls for numerical means to solve them. However, some simple problems may be solved by the inverse method. In this method, we ﬁrst assume a suitable form for the deformation and then use the constitutive equations to ﬁnd the associated stresses and consider the restrictions imposed by the equations of equilibrium. Finally, we determine the surface tractions necessary to maintain the deformation. These simple problems serve to illustrate the method of solution in ﬁnite elasticity, and some of these problems have added importance in that they may be experimentally investigated. They are then used to determine the form of the strain-energy function of a given elastic material. The following

© 2005 by Chapman & Hall/CRC Press

186

Continuum Mechanics and Plasticity

two forms of the strain-energy function are well known. They are W = C(I1 − 3)

(4.179)

W = C1 (I1 − 3) + C2 (I2 − 3)

(4.180)

and

in which C, C1 , and C2 are constants. Form (4.179) is known as the Neo-Hookean form which was derived from kinetic theory of rubber by Treloar. Form (4.180) is known as the Mooney form or the Mooney–Rivlin form. Following Rivlin [3], the strain-energy function W = W (I1 , I2 , I3 ) of an isotropic material, which is normally expressed in a polynomial of I1 , I2 , and I3 , may be equally expressed as a polynomial function of (I1 − 3), (I2 − 3), and (I3 − 1). Thus,

W=

Aαβγ (I1 − 3)α (I2 − 3)β (I3 − 1)γ

(4.181)

α,β,γ

where Aαβγ are constants. When the material is undeformed, C11 = C22 = C33 = 1, and I1 − 3 = 0, I2 − 3 = 0, I3 − 1 = 0. Following this approach, the strain-energy function for incompressible material is given by W=

Aαβ (I1 − 3)α (I2 − 3)β

(4.182)

α,β

4.8.4.1 Uniaxial extension In the case of uniform extensions, the deformation is given by (3.18). Using (3.18), we ﬁnd

λ21

[B] = 0

0

0

0

λ22

0 ,

0

λ23

λ41

[B2 ] = 0

0

0

0

λ42

0

0

λ43

(4.183)

Substituting (4.183) into (4.177), we obtain σ11 = 2{W1 λ21 + W2 (I1 λ21 − λ41 ) − p}

(4.184a)

σ22 = 2{W1 λ22 + W2 (I1 λ22 − λ42 ) − p}

(4.184b)

σ33 = 2{W1 λ23 + W2 (I1 λ23 − λ43 ) − p}

(4.184c)

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

187

For uniaxial test, σ22 = σ33 = 0. Using these conditions and subtracting (4.184b) from (4.184a), we obtain σ11 = 2{W1 (λ21 − λ22 ) + W2 [I1 (λ21 − λ22 ) − (λ41 − λ42 )]}

(4.185)

which reduces to σ11 = 2(λ21 − λ22 ){W1 + W2 (I1 − λ21 − λ22 )}

(4.186)

σ11 = 2(λ21 − λ22 ){W1 + λ23 W2 }

(4.187)

or

The expression I1 = λ21 + λ22 + λ23 was used to arrive at this equation. In addition, by subtracting (4.184c) from (4.184b), we obtain 0 = 2(λ22 − λ23 ){W1 − λ21 W2 }

(4.188)

This quantity must vanish for all λ1 and, therefore, λ2 = λ3 . If the material is incompressible, then det F = 1, so that λ1 λ22 = 1

with λ2 = λ3

(4.189)

Hence, by substituting (4.189) into (4.187), we obtain 1 + W = 2 W 1 2 λ1 λ21 − (1/λ1 ) σ11

(4.190)

In the experiments of uniaxial tension and compression, σ11 and λ1 may be measured and the left-hand side of (4.190) may be calculated. The details of the experiments are reported in Rivlin and Saunders [4] from vulcanized rubber test-pieces. The experimental results show that when σ11 /(λ21 − λ−1 1 ) is plotted against 1/λ1 , the material response for the case of 1/λ1 < 1 (tension) is quite different from that for the case of 1/λ1 > 1 (compression). The experimental data in the tension zone and in the compression zone can be best ﬁtted by the Mooney form (4.180) and the Neo-Hookean form (4.179), respectively. Figure 4.8 shows a schematic plot of the two models each applied in the recommended zone. 4.8.4.2

Simple shear

The simple shear deformation has been previously discussed in Section 3.4.1.2 and Example 3.3. The transformation equations for this deformation are x1 = X1 + kX2 ,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(4.191)

188

Continuum Mechanics and Plasticity

Tension

– 2 1

11

–1 1

Compression Neo-Hookean form

ey on Mo m for

1/1

1.0 FIGURE 4.8 Uniaxial tension and compression.

where k is a nonzero constant, and, based on (4.191), we ﬁnd

1 + k2 [B] = k 0

k 0 1 0 0 1

1 [B−1 ] = −k 0

−k 1 + k2 0

0 0 1

(4.192)

with I1 = 3 + k 2 ,

I2 = 3 + k 2

and

I3 = 1

(4.193)

Thus, there is no change in volume during simple shearing. Using the hyperelastic constitutive equation (4.178), we ﬁnd σ11 = −p + 2(1 + k 2 )W1 − 2W2

(4.194a)

σ22 = −p + 2W1 − 2(1 + k 2 )W2

(4.194b)

σ33 = −p + 2W1 − 2W2

(4.194c)

σ12 = kµ(k 2 )

σ23 = σ31 = 0

(4.194d)

in which the hydrostatic pressure p is to be determined by the prescribed boundary conditions and µ(k 2 ) = 2(W1 + W2 )

(4.194e)

where µ(k 2 ) is usually referred to as the generalized shear modulus. We note that k is the shear strain, and when we reverse the direction of shear, we change the sign of the shear stress. This is satisﬁed only when µ(k 2 ) > 0. In the case of small deformations, it is known that the simple shear deformation can be maintained by applying only shear stresses without normal

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

189

stresses on the faces of the specimen. In a ﬁnite deformation, we inquire whether this is still true, for shear strain k = 0. By setting σ11 = σ22 = σ33 = 0, we obtain from (4.194) that −p + 2(1 + k 2 )W1 − 2W2 = 0 −p + 2W1 − 2(1 + k 2 )W2 = 0

(4.195)

−p + 2W1 − 2W2 = 0 Solving the set of equations in (4.195) for a nontrivial solution for −p, 2W1 , and −2W2 , the determinant of the coefﬁcient matrix has to be zero. Thus, 1 1 + k 2 1 1 1 1

1 1 + k 2 = k 4 = 0 1

(4.196)

We obtain from (4.196) that k = 0, which corresponds to no shear deformation and is in contradiction with the assumption that k = 0. On the other hand, the trivial solution of p = W1 = W2 = 0, from (4.194a–e), leads to µ(k 2 ) = 0 and σ12 = σ11 = σ22 = σ33 = 0, that is, the shear strain k = 0 gives rise to no stresses, in contradiction with experimental observations. We therefore conclude that the simple shear deformation cannot be maintained by applying only shear stresses on the faces of the specimen. Generally, normal stresses must also be applied. From (4.194), the mean stress is 1 3 σkk

= (−p + 2W1 − 2W2 ) + 23 k 2 (W1 − W2 )

(4.197)

When k, −p, W1 , and W2 are all nonzero, then (4.197) gives rise to a nonzero mean stress. If normal stresses are not applied, then the material element will either expand or contract in volume according to the sign of the mean stress. However, this deformation is not a simple shear deformation. From (4.194a–e), we may also obtain σ11 − σ22 = kσ12

(4.198)

This relation does not depend on the form of the strain-energy function. An implication of this equation is that during shearing, the normal stresses σ11 and σ22 cannot be equal. The existence of these unequal normal stresses is called the Poynting effect. This effect was ﬁrst investigated by Poynting [5] who performed a series of torsion experiments on metal wires and observed the lengthening of wires when no axial force was applied. This effect is also known as the axial effect and is discussed later related to plastic deformation. In order to maintain the simple shear deformation, normal stress σ N and shear stress σ S must be applied on the inclined faces of the deformed

© 2005 by Chapman & Hall/CRC Press

190

Continuum Mechanics and Plasticity 2

22 12

D

C

22 S

12 s

11

n

A

N 1

B

FIGURE 4.9 Simple shear.

specimen. These stresses are now calculated. Referring to Figure 4.9, the outward normal n to the inclined surface BC has components [n] = [cos γ , − sin γ , 0]

(4.199)

where the angle γ is deﬁned by k = tan γ , with sin γ = k/ 1 + k 2 and cos γ = 1/ 1 + k 2 . The unit tangential vector s has components [s] = [sin γ , cos γ , 0]

(4.200)

The normal and shear components are then

σ N = σij nj ni = [cos γ

− sin γ

σ11 0] σ12 0

σ12 σ22 0

0 cos γ 0 − sin γ σ33 0

= σ11 cos2 γ + σ22 sin2 γ − σ12 sin 2γ σ S = σij nj si =

(4.201)

(σ11 − σ22 ) sin 2γ + σ12 cos 2γ 2

(4.202)

Since sin 2γ = 2k/(1 + k 2 ), cos 2γ = (1 − k 2 )/(1 + k 2 ), and σ11 − σ22 = kσ12 , it is easily shown that σ N = σ22 − kσ S

and

σS =

σ12 1 + k2

(4.203)

We now see that σ S < σ12 and σ N < σ22 . This assures that if σ22 is in compression and is negative, so is σ N in compression.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

191

F

F

2

1 3 FIGURE 4.10 Biaxial compression of a cubic block.

EXAMPLE 4.10

Find the state of stress in the biaxial compression of a cubic

block. Solution This test is sometimes referred to as the conﬁned compression test. Referring to Figure 4.10, the block is conﬁned in the 2-direction, while a compressive force F is applied in the 1-direction. The 3-direction is free. The deformation is governed by x1 = λ1 X1 ,

x2 = λ2 X2 ,

x3 = λ3 X3

(a)

and we ﬁnd from (a)

λ1 [F] = 0 0

0 λ2 0

0 0 , λ3

λ21

0

0

[B] = 0

λ22

0 ,

0

0

λ23

λ41

0

0

[B2 ] = 0

λ42

0

0

0

λ43 (b)

with |F| = λ1 λ2 λ3 = λ1 λ3 = 1. We used λ2 = 1, since the block cannot deform along the 2-direction. The stresses are found by putting (b) into (4.177), which leads to (4.184a–c). Because the 3-direction is free, we write σ33 = 0. Using this constraint, (4.184c) becomes p = W1 λ23 + W2 (I1 λ31 − λ43 )

(c)

Substituting (c) into (4.184a), we then obtain σ11 = 2{W1 λ21 + W2 (I1 λ21 − λ41 ) − W1 λ23 − W2 (I1 λ23 − λ43 )}

© 2005 by Chapman & Hall/CRC Press

(d)

192

Continuum Mechanics and Plasticity

The ﬁrst invariant of B is I1 = λ21 + λ22 + λ23 = λ21 + 1 +

1

(e)

λ21

Applying (e), (d) may be further reduced to λ21

σ11 = 2

−

1

{W1 + W2 }

λ21

(f)

Similarly, we obtain the following equation from (4.184b) σ22 = 2 1 −

1

{W1 + W2 λ21 }

λ21

(g)

For the Neo-Hookean form given by (4.179), W1 = C and W2 = 0. The stresses are found from (f) and (g) as σ11 = 2

λ21

−

1 λ21

σ22 = 2 1 −

C,

1

λ21

C = constant

C,

(h)

From (h), we ﬁnd the following stress ratio which indicates a conﬁned stress in the 2-direction ξ=

1 σ22 = σ11 1 + λ21

(i)

Equation (i) is plotted against λ1 in Figure 4.11. We note that ξ = 1.0 when λ1 = 0; ξ = 0.5 when λ1 = 1; and ξ = 0 when λ1 → ∞. For the Mooney form given by (4.180), W1 = C1 and W2 = C2 . The stresses are found from (f) and (g) as σ11 = 2

λ21

−

1 λ21

{C1 + C2 },

σ22 = 2 1 −

1 λ21

C1 , C2 = constants

C1 + C2 λ21 , (j)

From (j), we ﬁnd the following stress ratio ξ=

C1 + C2 λ21 σ22 = σ11 (1 + λ21 )(C1 + C2 )

(k)

We see from (k) that ξ = C1 /(C1 + C2 ) when λ1 = 0; ξ = 0.5 when λ1 = 1; and ξ = C2 /(C1 + C2 ) when λ1 → ∞. The exact shape of the curve depends on the values of C1 and C2 . In a special case when C1 = C2 , we obtain ξ = 0.5 for

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

Neo-Hookean Mooney

1

0.5

193

C1 C1 + C2 C2 C 1 + C2

0

0.5

1

Compression

1.5

2

1

Tension

FIGURE 4.11 The ξ ratio plotted against λ1 .

all λ1 . According to Rivlin and Saunders [4], W1 > W2 for vulcanized natural rubber, and, therefore, C1 > C2 . Equation (k) is plotted in Figure 4.11 for the case of C1 = 2.5C2 (C1 > C2 ). We note that the conﬁning stress σ22 is always smaller than σ11 for both models. They are equal only in the Neo-Hookean model when λ1 = 0, which is a limiting case and cannot realistically happen.

4.9 4.9.1

Inﬁnitesimal Theory of Elasticity Constitutive Equation

We showed in Section 3.9.1 that, in the case of small displacement gradient, it is not necessary to distinguish the material coordinates XR from the spatial coordinates xi . Thus, the inﬁnitesimal strain tensor εij = 12 (ui,j + uj,i )

(4.204)

can and will be used. In this case, both Lagrangian strain E and Enlerian strain e reduce to ε. There are no distinctions among different stress measures and σij is used to denote the stress which is also known as the engineering stress. To show that this is indeed the case, we denote the magnitude of the displacement gradient by ε = (ui,R · ui,R )1/2

(4.205)

We use the notation ε to indicate that this is a small quantity, and it should not be confused with the strain ε used in Chapter 3. The deformation gradient is FiR = δiR + ui,R = δiR + O(ε)

© 2005 by Chapman & Hall/CRC Press

(4.206)

194

Continuum Mechanics and Plasticity

where O(ε) indicates that the magnitude of this term has the order of ε. The determinant is |FiR | = det(δiR + ui,R ) = 1 + O(ε) + O(ε 2 ) + O(ε 3 )

(4.207)

ρ0 = ρ|FiR | = ρ(1 + O(ε) + O(ε 2 ) + O(ε 3 ))

(4.208)

Thus,

On the other hand the inverse deformation gradient F−1 is XR,i = δRi − uR,i = δRi − O(ε)

(4.209)

so that from (4.42) and (4.48) the Piola–Kirchhoff stresses are related to σij by (0)

TRi =

ρ0 ∂XR = (1 + O(ε) + · · · )(δRj − O(ε))σji σji ρ ∂xj

(4.210)

and

RS =

ρ0 ∂XR ∂XS = (1 + O(ε) + · · · )(δRj − O(ε))(δSk − O(ε))σjk (4.211) σjk ρ ∂xj ∂xk

In the limit, when ε → 0, we have (0)

TRi ≈ (δRj − O(ε))σji ≈ σRi

(4.212)

RS ≈ (δRj δSk + O(ε))σjk ≈ σRS

(4.213)

which show that the 1st and 2nd P–K stresses are indistinguishable from σij . The constitutive equation for inﬁnitesimal theory of elasticity at room temperature may be obtained by taking the strain-energy function W (εij ) in a quadratic form, that is, W = 12 Cijkl εij εkl

(4.214)

By differentiation of (4.214) with respect to εij , we obtain σij =

∂W = Cijkl εkl ∂εij

(4.215)

Equation (4.215) is known as the generalized Hooke’s law, where Cijkl is a fourth-rank tensor. If the material is isotropic, then Cijkl should be an isotropic tensor, that is, from (1.129) Cijkl = λδij δkl + µ(δik δjl + δil δjk )

© 2005 by Chapman & Hall/CRC Press

(4.216)

Conservation Laws and Constitutive Equation

195

By combining (4.215) and (4.216), we then obtain σij = λδij εkk + 2µεij

(4.217)

where λ and µ are Lamé constants. Note that the number of material constants has been reduced from 81 to 2. Equation (4.217) may be inverted to express strain in terms of stress. To this end, we make a contraction of (4.217) to get σii = 3λεii + 2µεii = (2µ + 3λ)εii

(4.218)

so that (4.218) may be solved for εii and substituted into (4.217) to obtain σij =

λσkk δij + 2µεij 2µ + 2λ

(4.219)

Finally, we rewrite (4.219) as 2µεij = σij −

λ σkk δij 3λ + 2µ

(4.220)

This is the equation that we wanted to derive.

4.9.2

Homogeneous Deformations

4.9.2.1 Hydrostatic stress Consider the strain

ε11 εij = 0 0

0 ε22 0

0 0 ε33

(4.221)

In the case of hydrostatic stress, ε11 = ε22 = ε33 = α. Substituting into (4.217), the stress is σij = (2µ + 3λ)αδij = −pδij

(4.222)

P = −(2µ + 3λ)α

(4.223)

Therefore,

and the volumetric strain is εkk = 3α =

© 2005 by Chapman & Hall/CRC Press

−3p −p σkk = = 3K 3K K

(4.224)

196

Continuum Mechanics and Plasticity

where K is the bulk modulus and σkk /3 is the mean stress. Thus, by use of (4.223), K=

−p −p 2 = =λ+ µ 3α (−3p)/(2µ + 3λ) 3

(4.225)

Note that since a hydrostatic pressure always causes the volume to decrease (α < 0), we have K > 0. In the case that p < 0, the volume expands and it is known as dilation. 4.9.2.2 Uniaxial tension When σ11 = σ22 = 0 and σ33 = 0, Hooke’s law reduces to σ11 = 2µε11 + λ(ε11 + ε22 + ε33 ) = 0 σ22 = 2µε22 + λ(ε11 + ε22 + ε33 ) = 0

(4.226)

σ33 = 2µε33 + λ(ε11 + ε22 + ε33 ) Comparing the ﬁrst two equations of (4.226), we ﬁnd λ (ε33 + 2ε22 ) 2µ

(4.227)

λ ε33 = −νε33 2(λ + µ)

(4.228)

ε11 = ε22 = − which may be solved to obtain ε11 = ε22 = − where ν=

1 λ 2λ+µ

(4.229)

is Poisson’s ratio. By substituting these expressions into the third equation of (4.226), we obtain σ33 = 2µε33 + λ(1 − 2ν)ε33 = (2µ + λ − 2νλ)ε33 λ2 µ(3λ + 2µ) = 2µ + λ − ε33 = ε33 = E ε33 λ+µ λ+µ

(4.230)

where E = µ(3λ + 2µ)/(λ + µ) is known as Young’s modulus. In an elastic material, E > 0 and ν > 0.

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

197

4.9.2.3 Simple shear In the inﬁnitesimal deformation, simple shear does not give rise to normal stresses. The nonzero strain components are ε12 = ε21 only. From (4.217), the shear stress is σ12 = 2µε12

(4.231)

where µ > 0 is the shear modulus. The engineering shear strain is 2ε12 .

4.9.3

Boundary-Value Problems

In solving boundary-value problems of isothermal inﬁnitesimal elasticity, the fundamental equations are the equations of motion, σki,k + bi = ρ

D2 ui Dt2

(4.232)

the constitutive equations, σij = λδij εkk + 2µεij

(4.233)

and the strain–displacement relation, εij = 12 (ui,j = +uj,i )

(4.234)

There are three equations in (4.232), six equations in (4.233) and six equations in (4.234), and the unknowns are σij , εij , ui . We have 15 equations to solve for 15 unknowns. In ﬁnding the solution, the boundary conditions should be used. There are three types of boundary-value problems: the displacement boundary-value problems have ui speciﬁed on the boundary S; (n) the traction boundary-value problems have the stress vector ti speciﬁed on S; and the mixed boundary-value problems have ui speciﬁed on part of S (n) and ti speciﬁed on the remaining part of S. The surface traction is given, from (2.8), by (n)

ti

4.10

= σji nj

(2.8)

Hypoelasticity

Hypoelasticity is not elasticity, because the stress in hypoelasticity depends on the strain-path. This type of constitutive equation is popular in computational mechanics as it is of the rate-type. The rate-type equations have

© 2005 by Chapman & Hall/CRC Press

198

Continuum Mechanics and Plasticity

advantages over other types of equations due to the ease in numerical computation. We ﬁrst write the generalized Hooke’s law (4.217) of the inﬁnitesimal elasticity in the rate form as

σ˙ ij = 2µ˙εj + λδij ε˙ kk

(4.235)

and then inquire what the corresponding constitutive equation should be for ﬁnite deformation. We learned at the beginning of this chapter that objective rates need to be used in a constitutive equation. The Jaumann stress-rate is a popular objective stress rate and is used together with the rate of deformation tensor, so that an appropriate hypoelastic constitutive equation is written as σij∇ = 2µDij + λδij Dkk

(4.236)

A discussion using other objective stress-rates is given in Chapter 7 in connection with the study of plastic deformation. We discuss now a simple example using (4.236). Let us consider simple shear having the following equations x1 = X1 + 2ωt X2 , u1 = 2ωt X2 ,

0 [L] = 0 0

2ω 0 0

0 0 , 0

x2 = X2 ,

u2 = u3 = 0,

ω 0 0

0 [D] = ω 0

x3 = X3

(4.237)

ω = constant 0 0 , 0

0 [W ] = −ω 0

(4.238) ω 0 0

0 0 0 (4.239)

Substituting (4.239) into (4.236), we ﬁnd σij∇ = 2µDij

and

Dkk = 0

(4.240)

But the Jaumann rate is σ∇ =

Dσ − W · σ + σ · W = 2µD Dt

(4.241)

For the stress given by

σ11 [σ ] = σ12 0

© 2005 by Chapman & Hall/CRC Press

σ12 σ22 0

0 0 0

(4.242)

Conservation Laws and Constitutive Equation

199

we can compute the following matrices

−ωσ12 ωσ11 [σ ][W ] = −ωσ22 ωσ12 0 0 −ωσ12 −[W ][σ ] = ([σ ][W ])T = ωσ11 0

0 0 , 0 −ωσ22 ωσ12 0

0 0 0

(4.243)

Substituting (4.242) and (4.243) into (4.241), the component equations are dσ11 = 2ωσ12 , dt

dσ22 = −2ωσ12 , dt

dσ12 = 2µω − ω(σ11 − σ22 ) (4.244) dt

Note that D/Dt = d/dt in this homogeneous deformation. By differentiating (4.244c) with respect to t and making use of (4.244a,b), we obtain the ordinary differential equation d2 σ12 = −4ω2 σ12 dt2

(4.245)

The general solution of (4.245) is σ12 = A sin(2ωt) + B cos(2ωt) where A and B are constants. We deﬁne the shear strain by γ = during loading, the shear strain is

(4.246) t 0

D12 dt, and,

γ = 2ωt

(4.247)

Note that γ is not a component of a strain tensor. By taking the initial shear stress to be σ12 (t = 0) = 0, we ﬁnd from (4.246) that B = 0. Therefore, we obtain the following stress components σ12 = µ sin γ ,

σ11 = −σ22 = µ(1 − cos γ ),

other σij = 0

(4.248)

It can be seen from (4.248) that the shear and axial stresses oscillate with the increasing shear strain, and these are physically unacceptable with any real material. Nagtegall and de Jong [6] discussed this oscillatory behavior of the shear stress in his application of a plasticity model. The work triggered a longlasting investigation of objective stress rates by various investigators, and the subject is discussed further in Chapter 7 in connection with ﬁnite plasticity. Equations of (4.248) are plotted in Figure 4.12 with µ = 26.2 GPa, which is a typical value for cast high-purity aluminum.

© 2005 by Chapman & Hall/CRC Press

200

Continuum Mechanics and Plasticity Stress (MPa)

40 20 –4

2

–2

4

–20 –40 –60

12 22

FIGURE 4.12 Hypoelastic stress–strain curves by use of Jaumann stress rate.

References 1. Rivlin, R.S. and Ericksen, J.L., Stress–deformation relations for isotropic materials, J. Ration. Mech. Anal., 4, 323, 1955. 2. Green, A.E. and Adkins, T.E., Large Elastic Deformations, Oxford University Press, Oxford, 1960, 7. 3. Rivlin, R.S., Some topics in ﬁnite elasticity, in Proc. 1st Symp. Naval Structural Mech., Goodier, J.N. and Hoff, N.J., Eds., 1958, 169. 4. Rivlin, R.S. and Saunders, D.W., Large elastic deformations of isotropic materials VII. Experiments on the deformation of rubber, Phil. Trans. R. Soc. Lond., A243, 251, 1951. 5. Poynting, J.H., On pressure perpendicular to the shear planes in ﬁnite pure shears, and on the lengthening of loaded wires when twisted, Proc. R. Soc., A82, 546, 1909. 6. Nagtegall, J.C. and de Jon, J.E., Some aspects of non-isotropic workhardening in ﬁnite strain plasticity, in Proc. Workshop on Plasticity of Metals at Finite Strain: Theory, Experiment and Computation, Lee, E.H. and Mallet, R.L., Eds., Stanford University, 1981, 65.

Problems (1) Consider uniform extension of a material element followed by simple shearing. In the uniform extension along the X2 direction, a particle at X is displaced to X by X1 = β(t)X1 , X2 = α(t)X2 , X3 = β(t)X3

© 2005 by Chapman & Hall/CRC Press

Conservation Laws and Constitutive Equation

201

The subsequent simple shearing is expressed as x1 = X1 + 2η(t)X2 ,

x2 = X2 ,

x3 = X3

where 2η(t) is the shear strain after the uniform extension. Find the components of the 1st and 2nd P–K stresses expressed in terms of the Cauchy stress components. (2) For isotropic hyperelastic materials, show that the principal axes of the Cauchy stress and the left Cauchy–Green tensor coincide. (3) Consider a compressible isotropic hyperelastic material. For the deformation given by x1 = α(t)X1 ,

x2 = α(t)X2 ,

x3 = α(t)X3

discuss the corresponding state of stress. Obtain an expression for the stress vector and discuss the volume change of the material element. (4) Discuss the simple shear problem by means of Cauchy elasticity, that is, σij = χ0 δij + χ1 Bij + χ−1 B−1 ij where χ0 , χ1 , and χ−1 are functions of I1 , I2 , and I3 . (5) Find the state of stress in the biaxial compression of a cubic block discussed in Example 4.10, if the strain-energy function is given by W=

i

C1 (λ2i − 1) + C2

1 λ2i

−1

where C1 and C2 are constants and λi are the stretch ratios. (6) Find the state of stress in the simple torsion of a circular cylinder of incompressible hyperelastic material with length l and radius a. The deformation of this problem is expressed by x1 = (cos τ X3 )X1 − (sin τ X3 )X2 , x2 = (sin τ X3 )X1 + (cos τ X3 )X2 , x3 = X3 where τ is the angle of twist per unit length and is a constant.

© 2005 by Chapman & Hall/CRC Press

Part II

Continuum Theory of Plasticity Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (continuum) approach is still the practical approach for use in the simulation of engineering problems.

© 2005 by Chapman & Hall/CRC Press

5 Fundamentals of Continuum Plasticity

5.1

Introduction

A general description of plasticity is given in this chapter. Plastic deformation can be easily observed by stretching a thin copper wire. If we stretch a piece of copper wire beyond its elastic limit, then we observe a permanent change in length of the copper wire after the release of the load. This is because the wire is permanently elongated and has undergone a plastic deformation. The copper wire is very soft and easily stretched by a small force. The elastic limit of the material (copper) can be easily exceeded. In this onedimensional case, the experimental stress–strain curve for copper is sketched in Figure 5.1. We use this ﬁgure to illustrate properties and terminologies of plastic deformation. When the stress increases from O to A, the strain also has a proportional increase. The process of increasing the stress is known as loading. The initial yielding of the material occurs at A and the stress at this point is known as the yield stress and is denoted by σy . The yield stress is generally regarded as equal to the elastic limit, but the elastic limit and the proportional limit are experimentally indistinguishable for metals. Several deﬁnitions of yield stress have been proposed and they are discussed in Chapter 6. Should the stress be reduced from A back to O, we have an unloading process. OA is the elastic region and the Hooke’s law applies in this region. All strains within the elastic region are recovered upon unloading and are elastic strains. Point A is the ﬁrst point beyond which nonrecoverable strain occurs. This strain is permanent and is known as the plastic strain, which is either time-independent or time-dependent. In plasticity, we are interested in the time-independent nonrecoverable strain. The time-dependent nonrecoverable strain is related to creep. The curve OABE is the stress–strain curve for monotonic loading. The initial yielding of material occurs at A and yielding continues as the curve ABE is traversed. The strain at B is ε, which can be divided into the elastic ε e and plastic εp parts, where ε = εe + εp

(5.1) 205

© 2005 by Chapman & Hall/CRC Press

206

Continuum Mechanics and Plasticity

y

E

B

A

F Ο

p

e C

G

D FIGURE 5.1 Schematic stress–strain curve for Cu and Al.

The elastic and plastic strains for point B are shown in Figure 5.1. Curves BCD and EFG are unloading stress–strain curves. The initial part of the unloading curves is straight and the curves gradually bend over. In the ﬁgure, sections BC and EF are straight with slopes similar to that of section OA. Generally, for a good approximation, these slopes are assumed to be equal. But, experimental data show that the unloading slope depends on the strain level where the unloading begins to take place. Thus, EOA > ECB > EFE , that is, the slope is smaller if unloading occurs at a higher strain level. C and F are points of reverse yielding. Usually, the reverse yielding can occur on the compressive stress side as in point C, but as the strain at which unloading takes place gets higher, the reverse yielding occur on the tension side as in point F. The effect of the decrease in the yield stress in the reverse loading, that is, |σyC | < |σyB |, is known as the Bauschinger effect and it is an anisotropic hardening. The description of the stress–strain curve presented above is based on experimental observations and data. An enormous challenge in plasticity is to formulate a realistic mathematical model for describing the observed material behavior. The task is known as constitutive modeling and the end product is a constitutive model or a set of constitutive equations. Various theories using different approaches and points of views have been proposed to formulate constitutive equations for metallic materials. Theories have also been formulated based on dislocations and slips. Although physically based polycrystal plasticity is emerging as a feasible method, the phenomenological (or continuum) approach is still the practical approach for use in the computational mechanics. Presently, there are great research efforts aiming to bridge the gap between mechanics at microscopic and continuum level. Some exciting results have already been reported and they provide input to the continuum theory of plasticity. Some of these inputs are discussed in Chapter 7 in connection with ﬁnite plasticity. In spite of the interest in plasticity at the microscopic level, the continuum theory is still the backbone for the study of plasticity.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

207

In this book, we discuss the continuum approach of plasticity. Most of our discussions are related to the plastic deformation of metals, although some may be applicable to other materials as well. In the study of plasticity, theories and experiments have gone hand-in-hand. Experimental results have led to the development of theories and theoretical studies have suggested new experiments. The ultimate goal is to develop a theory of plasticity that can be experimentally veriﬁed. Experimental results have been greatly inﬂuenced by the loading equipment and measuring technology. Problems associated with the loading equipment are the stiffness of the loading machine and the kind of the loading machine. Is it a dead-weight machine or is it a servo-controlled hydraulic testing system? Older data were gathered by use of dead-weight machine. Deadweight machines have an advantage in providing steady, well-controlled load increments and it can be used to obtain creep strains, but it cannot be used to execute a strain-controlled test program. Some dead-weight machines have cross-talks, that is, the axial load is inﬂuenced by the torsion load and vice versa in an axial–torsion test machine, resulting in inaccurate experimental results. Most commercially available servo-hydraulic machines have acceptable cross-talk level. An important advantage of the servo-hydraulic machines is that it is fully automated and it can execute either a strain-controlled or a stress-controlled test program. Due to the nature of the closed-loop servocontrolled machine, the data scatter to an extent which depends on the time interval of data acquisition. This data scatter may affect the accuracy of the data collected. Some examples that are sensitive to this data scatter are Young’s modulus of the stress–strain curve and yield stresses. These effects are further discussed in a later section. The strain can be measured by measuring the motion (displacement and rotation) of the cross-heads of the test machine. This method of measurement is, however, inﬂuenced by the stiffness of the machine and the shape of the specimens. Let L and φ, respectively, be the displacement and rotation of the cross-heads, r be the radius of a cylindrical specimen and L be the length of the specimen between the grips, then the axial strain ε and shear strain γ , respectively, are written as ε = L/L and γ = rφL. Since L includes the lengths of the enlarged gripping sections and the uniform gauge section of the specimen, the strains determined by use of the above expressions represent the average strains of the specimen and do not accurately represent the strains of the gauge section. It is the strains of the gauge section that are meaningful. The stiffness of the machine is not a factor, if we directly measure the strains in the gauge section of the specimen. Extensometers or strain gauges may be used to accomplish the job. Extensometers may be self-designed and is also available commercially. The resolution of extensometers is around 10−3 strain, but it can measure strains of up to about 15%. Extensometer for larger strains needs to be self-designed. Wu and Xu [1] built an axial–torsion extensometer that may be installed and clipped on the uniform gauge section of the specimen. Shear strains of up to 200% have been measured by Wu et al. [2]

© 2005 by Chapman & Hall/CRC Press

208

Continuum Mechanics and Plasticity

using this extensometer. Electrical-resistance strain gauges and strain rosettes are commercially available and they are easy to use. The resolution for this type of strain gauges is around 10−6 and it therefore provides much more accurate strain measurements than the extensometers. But, these gauges are limited to a strain of around 2% and either peel off or broken beyond 2% strain. A post-yield type strain gauge is available and it can measure axial strains of up to around 15%. No post-yield strain-rosettes are as yet commercially available. To design an experiment and collect valid data is a challenge and must be carefully pursued. The extension of one-dimensional plasticity into a multi-dimensional plasticity provides an even greater challenge both experimentally and theoretically. In the early development, two major schools of thought were developed; the ﬂow theory and the deformation theory. The deformation theory was proposed by Hencky in 1924 and the approach was used thereafter by Russian researchers. The Hencky equation is εij =

kσkk δij + ψsij 3

(5.2)

where k and ψ are scalars. We note that the total strain εij rather than the strain increment dεij is found from (5.2) and, therefore, the deformation theory is also known as the total strain theory. On the other hand, the ﬂow theory emphasizing the strain increment is also known as the incremental theory. The deformation theory is convenient for use, due to mathematical simplicity, in solving problems with proportional loading. The ﬁnal state of strain is determined by the ﬁnal state of stress. However, it is known that the equations of deformation theory are not suitable for nonproportional loading condition and the deformation theory will not be further pursued in this book. In this chapter we describe the fundamentals of plasticity from an experimentalist’s view point. The concepts of ﬂow theory is discussed in Chapter 6. The major concepts of ﬂow plasticity are: the yield surface, the ﬂow rule, the strain-hardening rule, and the loading–unloading conditions. Experimental evidence is presented together with the mathematical representations and assumptions of the theory are discussed. One of the major assumptions is the plastic incompressibility of metallic materials. Recent developments in plasticity are given in Chapter 7. It includes experimental and theoretical developments both for inﬁnitesimal and ﬁnite plasticity. Other developments, such as the endochronic theory, are discussed in Chapters 8 and 9. The author has been involved in the development and veriﬁcation of this theory, and a detailed account of the theory is given. The thermo-mechanical theory of internal state variables is ﬁrst presented in Chapter 8 and the presentation of the endochronic theory follows. The endochronic theory is an internal variables theory. Material anisotropy is an important topic of plasticity. The anisotropic properties of metal sheets are discussed in Chapter 10 and, in Chapters 11 and 12, we present a general theory of anisotropic plasticity. Since a square material element in the reference conﬁguration gets distorted by deformation,

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

209

curvilinear coordinates must be used and the stress and strain refer to this distorted element. In this way, we investigate the change in properties of the same material mass.

5.2

Some Basic Mechanical Tests

In this section, we discuss some basic experiments used to characterize the mechanical behavior of a material. They include the uniaxial tension test, uniaxial compression test, torsion test, and the creep test. These are onedimensional tests and aimed to produce axial and shear stress–strain curves and creep curves. They are very simple theoretically, but it is not so simple experimentally to obtain valid data. We refer to Bell [3] for a detailed account of experiments carried out during the ﬁrst half of the 20th century.

5.2.1

The Uniaxial Tension Test

Uniaxial tensile testing can be carried out quickly and easily and is used to measure the strength and ductility of materials. The specimens for tension test can be round or ﬂat specimens and they consist of enlarged end sections and a reduced gauge section. The round specimens can have threaded ends for gripping and the ﬂat specimens can either be with or without a pin-hole for connection to the load-train. The longer the gauge section is the more accurate the test results will be. The general shape of the loading stress–strain curve shown in Figure 5.1 is typical of those for aluminum, copper, brass, 304 stainless steel, and highstrength steels such as AISI 4142 steel in the small strain range, that is, when the strain is 50% before necking. Thinning of a sheet specimen can occur at a strain ·2 > ·1

·2 > ·1

(c)

T1

T2 T3

T3 > T2 > T1

FIGURE 5.9 (a) Schematic constant strain-rate stress–strain curves, (b) constant strain-rate stress–strain curves for mild steel, (c) the effect of temperature.

A

A

B C

O

A

FIGURE 5.10 Loading stress–strain curve, creep, and stress relaxation.

Some fundamental concepts of strain-rate effect are constant strain-rate stress–strain curves as previously discussed, creep, and stress relaxation. Creep is the deformation developed as time elapses when the applied stress is kept constant. On the other hand, when the strain is kept constant, the stress relaxes with time. In Figure 5.10, OA shows the loading stress–strain curve; AB shows that the strain creeps from A to B while the stress is kept constant at σA ; and AC shows that the stress relaxes from A to C while the strain is kept constant at εA . A typical creep curve is a plot of strain against time and it is divided into three stages: the primary creep, the secondary creep,

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

227

D B

C

A

O

t

FIGURE 5.11 A schematic creep curve with three stages.

and the tertiary creep, as shown in Figure 5.11. The primary creep (also known as the transient creep) (AB) occurs at the beginning of the creep process. During this stage, the creep rate decreases continually. The creep rate remains nearly constant in the secondary (or steady state) creep stage (BC), and the creep rate increases continually until rupture during the tertiary creep stage (CD). It is convenient to separate the creep into three stages. However, no observations are available that show creep to be completely separated into three independent stages. It takes a long time to reach the tertiary stage; tertiary stage begins after 1940 h of creep, for instance, for an austenitic stainless steel tested at 704◦ C under a stress of 90.9 MPa (13,200 psi) [23]. The creep curves are dependent on the hold stresses. The higher the hold stress, the larger is the creep strain. Creep tests conducted at constant load or constant stress also give different creep curves. In the past (before about 1980), plastic deformation and creep were investigated separately. Experiment to determine plastic behavior was performed by use of screw-driven universal testing machines and creep experiment was conducted by dead load machines. An accurate control of rate of loading or rate of straining was difﬁcult in both cases. This method of experimental investigation gave rise to separate theories for plastic deformation and creep behavior. In this manner, the inelastic strain consists of a time-independent plastic strain term and a time-dependent creep strain term; these terms are calculated using plasticity and creep theories, respectively. Recently (after about 1980), new type servo-controlled testing equipment permits an accurate control of rate of loading or straining under quasi-static condition. It provides the means of recording the nonlinear, inelastic behavior of materials in detail and with great accuracy. The machine is so powerful that interactions between plasticity and creep can also be investigated. In this connection, we are interested in the primary and secondary creep stages. It is difﬁcult to draw a line between the two stages as previously mentioned and we will show continuous creep curves. Some interaction phenomena that have been reported are: the cyclic hardening or softening with hold time;

© 2005 by Chapman & Hall/CRC Press

228

Continuum Mechanics and Plasticity

the effect of creep prestrain on the subsequent plastic behavior; and the effect of plastic strain on the subsequent creep behavior. Corum et al. [24] showed that the stress amplitude in the cyclic tension–compression tests with a constant strain amplitude was enhanced by the preceding creep for AISI Type 304 stainless steel. Ikegami and Niitsu [25] found that SUS 304 stainless steel hardens in the direction of the preloading not only by plastic strain but also by creep strain. The hardening by creep is nearly equal to that by plastic strain. Wu and Ho [26] investigated strain hardening of 304 stainless steel by creep and found that the material hardened by creep is the same as that hardened by plastic deformation. Kujawski et al. [27], Wu and Yao [28], Wu and Ho [29], and Xia and Ellyin [30] observed that the creep curves are different even at the same holding stress but for different strain- or stress-rate loading histories prior to creep. In order to describe the aforementioned plasticity–creep interaction, recent efforts in material constitutive relation lean towards a uniﬁed theory for plasticity and creep. A fundamental issue of the creep test is the large range of data scatter. Some of the scatter may be attributed to the material inhomogeneities, but there are two other important factors contributing to the scatter. One factor is the test system misalignment and the other is the negligence of the pre-loading stage in a creep test by the investigators. These two factors are further explained. The misalignment in creep was investigated by Penny and Leckie [4] and Hayhurst [31]. These research workers generally agreed that data scatter in creep testing could be partially attributed to specimen alignment. Poor specimen alignment could result in bending stress (or strain) superimposed on the required mean axial stress (or strain). This bending stress (or strain) could be high enough to cause premature failure in brittle materials; in ductile materials, plastic deformation could occur and reduce the bending stress (or strain). Analyses of misalignment were presented by these investigators. The results show that the creep curves scatter due to eccentric loading. More signiﬁcantly, these analyses predicted that the scatter would increase with the creep time. The result of Wu and Wang [32] does not support all of the above assertions. Wu and Wang [32] considered the effect of pull-rods and the symmetric case of misalignment shown in Figure 5.3. The symmetric case is the most severe case of misalignment as discussed in [5]. It was pointed out in [32] that the following assumptions and/or conditions used by [4] and [31] are not realistic: (1) the applied load P is linearly related to the end moment M; (2) dP/dt = dM/dt = 0; (3) the neutral axis of the specimen is ﬁxed; and (4) the absence of pull-rod effect. The analysis of Wu and Wang [32] relaxed all of the aforementioned assumptions and led to different results as compared with [4] and [31]. While the numerical results of [32] show that the errors induced by the test system misalignment are signiﬁcant in the creep test, these errors will diminish with time. Thus, the most severe effect of misalignment occurs at the beginning of the creep test. Creep tests conducted with long pull-rods and large initial strain level (high creep stress) will tend to minimize the effect of misalignment.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

229

Another factor that is contributing to the scatter of creep data is the negligence of the preloading stage in a creep test. Due to the nature of dead load creep machines, the strain rate of the preloading stage in a traditional creep test is neither observable nor recordable. The way that the load (weight) is applied greatly affects the creep strain. Wu and Ho [29] conducted creep tests by use of a servo-controlled materials test system, and investigated the effect of the preloading stage on the subsequent creep. Two sets of test histories were used. One had a constant strain-rate preloading and the other had a constant stress-rate preloading. In the case with constant strain-rate preloading, the specimen was pulled in the strain-control mode while the computer monitored the strain and stress magnitude. The strain-rates were set at 2 × 10−6 , 10−5 , 10−4 , and 10−3 s−1 . As soon as the stress magnitude reached the preset creep holding stress, the loading process stopped. The test system was programmed to switch to the load-control mode instantaneously and then kept the stress at this constant magnitude, while the creep strain was being recorded. In the case with constant stress-rate preloading, the test was straightforward without control mode switching. The tests were performed under stress control at constant stress-rates of 2.07 and 20.7 MPa/s. As the stress reached the preset value, the creep process began. Each test result to be discussed was the average of two specimens. Most results were very consistent except for the case of constant strain-rate loading at 10−5 s−1 , where data scatter was apparent. A third test was conducted for this case and the result shown is the average of three tests. Two remarks can be made from the strain–time proﬁles of the whole creep process (the loading stage and the creep stage) shown in Figure 5.12, in which the starting point of the creep stage is marked by *. First, the proﬁles conﬁrm the constant strain-rate control of each curve prior to reaching the hold stress. Second, the proﬁles show that the initial creep strain rates are indeed a continuation of the preloading strain rates. Therefore, the initial creep strain rate of creep tests with strain-controlled preloading is known. Figure 5.13 shows the creep curves of various constant strain-rate preloading at the same holding stress of 206.7 MPa (30 ksi). For constant stress-rate preloading, the initial creep strain rate is also determined at the end of the loading stage. Thus, in the discussion of the creep stage, the initial creep rate is regarded as a known value. Figure 5.14 shows the strain–time proﬁles of the creep tests with constant stress-rate preloading. The starting points of the creep stage are marked by ∗ in the ﬁgure. It is seen that, during the preloading stage, the strain rate is constant in the elastic range and increases rapidly during elastic–plastic transition. The ﬁgure also shows that the initial creep strain rate is a continuation of the preloading strain rate. Figure 5.15 shows the creep curves for two creep tests with preloadings of two different constant stress rates. The hold stress for both tests was 206.7 MPa (30 ksi), same as the hold stress for the creep tests shown in Figure 5.13. In the elastic region, stress-rates of 2.07 and 20.7 MPa/s correspond to strain-rates of 1 × 10−5 and 1 × 10−4 s−1 , respectively. Because the initial creep rate of the creep test with faster stress-rate preloading is large, the corresponding creep

© 2005 by Chapman & Hall/CRC Press

230

Continuum Mechanics and Plasticity 2.5 1.e – 4 1.e – 5

2.0

2.e – 6 Total Strain (%)

1.e – 3 1.5

1.0

0.5

0

–0.5 0

50

100

150

200

Time (min)

Creep Strain (%)

FIGURE 5.12 Strain–time proﬁles of creep tests with various constant strain-rate preloading (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

–3

1.2

10

1

10

–4

0.8 –5

0.6

10

0.4

= 2 × 10

–6

0.2 10

20

30 40 Time (min)

50

60

FIGURE 5.13 Creep curves of various constant strain-rate preloading at the same hold stress (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

strain is larger than that of the creep test with a slower stress-rate preloading. Comparing creep curves of Figure 5.13 and Figure 5.15 with the same preloading strain-rate in the elastic region and having the same hold stress, the creep strains of constant stress-rate preloading approximately double those of constant strain-rate preloading. We may conclude that the preloading stage greatly affects the subsequent creep strain and that the traditional creep test using a dead load machine is vulnerable to data scatter, because neither the strain- nor the stress-rate of the loading stage can be controlled.

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

231

2.5

Total Strain (%)

2.0 1.5 1.0 20.7 MPa/s 2.07 MPa/s

0.5 0

–0.5 0

10

20

30 40 Time (min)

50

60

70

FIGURE 5.14 Strain–time proﬁles of creep tests with constant stress-rate preloading (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

Creep Strain (%)

20.7 MPa/s

1.5 2.07 MPa/s

1 0.5

10

20

30 40 Time (min)

50

60

FIGURE 5.15 Creep curves of two constant stress-rate preloading at the same hold stress (From Wu, H.C. and Ho, C.C., J. Eng. Mater. Technol., 117, 260, 1995. With permission from ASME).

5.3

Modeling the Stress–Strain Curve

For the purpose of applications and further theoretical studies, it is useful to develop a mathematical model for the one-dimensional stress–strain curve OABE shown in Figure 5.1. This is a generic stress–strain curve, it can be the curve for tension, compression, or shear. In 1909, Ludwik [33] proposed a stress–strain relationship to be used when the deformation was sufﬁciently

© 2005 by Chapman & Hall/CRC Press

232

Continuum Mechanics and Plasticity (a)

n = 0.5 n = 0.4 n = 0.3 n = 0.2 n = 0.1 n=0

2

/K

1.5 1 0.5

1

2

3

4

(b)

2.0 m=3 1.5

/y

m=5 m=9 m = 14 m = 30

1.0

0.5

1.0

2.0 3.0 /y

4.0

FIGURE 5.16 (a) The Ludwik equation, (b) the Ramberg–Osgood equation.

large so that the elastic strain could be neglected. The Ludwik equation is σ = Kεn

(5.37)

where K is a strength coefﬁcient and n is a strain-hardening exponent usually lying between 0 and 0.5. The equation predicts a zero initial stress and an inﬁnite initial slope, except for n = 0 which represents a rigid perfectly plastic material without strain-hardening. The higher the value of n, the more pronounced is the strain-hardening characteristic of the material. The Ludwik equation is plotted in Figure 5.16(a) for n = 0, 0.1, 0.2, 0.3, 0.4, and 0.5. If this equation is used to describe the plastic behavior and we combine the equation with Hooke’s law, which is used to describe the elastic behavior, the resulting equation can be used to describe the total material behavior. Writing the total strain as the sum of elastic and plastic parts, we obtain ε = εe + εp =

© 2005 by Chapman & Hall/CRC Press

σ σ 1/n + E K

(5.38)

Fundamentals of Continuum Plasticity

233

This equation, known as the Ramberg–Osgood Equation [34], is used by many investigators to express the monotonic loading curve of strain-hardening materials, especially ones without a sharply deﬁned yield stress. For a large number of metals, if the true stress is plotted versus the true plastic strain, a straight line results on a log–log plot and equation (5.38) proves useful. We rewrite (5.38) as ε σ = +α εy σy

σ σy

m (5.39)

where α=

E(σy )m−1 Km

and

m=

1 n

(5.40)

and σy and εy are the yield stress and yield strain, respectively, and related by σy = Eεy ; m is a hardening exponent; and α is a constant. Equation (5.38) is plotted in Figure 5.16(b) for α = 3/7 and m = 3, 5, 9, 14, and ∞. Note that (5.39) has three parameters. Other models have been proposed in the literature, but they will not be discussed here. Generally, the models describe similar curves using different mathematical expressions. Instead, we give some remarks related to the stress–strain curves in the large strain range. Many investigators specify that their equations relate the true stress to the true strain. The true strain is well deﬁned and the deﬁnition of true strain or logarithmic strain ε log has been discussed in Section 3.10. It may be shown from (3.139) that true strain is related to the engineering strain εeng by εlog = ln(1 + ε eng )

(5.41)

The true stress (or the Cauchy stress) is also well deﬁned and it is related to the nominal stress (or the 1st P–K stress) by (4.42). In the case of uniaxial stress for isotropic materials, the deformation gradient and stress components are

λ [F] = 0 0

0 λ2 0

0 0 , λ2

σ [σ ] = 0 0

0 0 0

0 0 , 0

s [T (0) ] = 0 0

0 0 0

0 0 0 (5.42)

Assuming that the material is incompressible at large strain, the Jacobian of the transformation is J = det F = λλ22 = 1

© 2005 by Chapman & Hall/CRC Press

(5.43)

234

Continuum Mechanics and Plasticity

Substituting (5.42) and (5.43) into (4.42), we obtain s=

σ = σ exp(−εlog ) λ

(5.44)

λ = exp(εlog )

(5.45)

where

Equation (5.44) has been used to convert the stress–strain curve expressed in terms of the true stress σ into that expressed in terms of the nominal stress and vice versa. In the tension test, the nominal stress is easily determined, because the initial cross-sectional area of the specimen is known. In this case, (5.44) is used to convert the nominal stress into the true stress. Both stress–strain curves are shown in Figure 5.17(a). Recently, some investigators have used diametral extensometers to measure the diametral strains in the cylindrical tension specimens. These diametral strains are then converted to the longitudinal strains based on a constant volume assumption. Let the volume be V = A0 l0 = Al, where A denotes the cross-sectional area and l the length of the specimen. The subscript 0 denotes the undeformed condition. If the volume remains constant, the differentiation of the above equation leads to dε

log

dA dl =− = l A

or

ε

log

A0 = ln A

(5.46)

The diametral strain is related to the change of area. The reduction of area deﬁned by (A0 − A)/A0 is often used. However, we need to remember that this approach is based on the constant volume assumption and it is a good approximation when the strain is large. In the compression test, the specimen is repeatedly remachined. The stress thus obtained is close to the true stress. We then use (5.44) to convert the true stress into the nominal stress. In doing so, we remark that the strain ε log is negative in compression. The stress–strain curves for compression are shown in Figure 5.17(b) plotting against the absolute value of the true strain.

5.4

The Effects of Hydrostatic Pressure

The hydrostatic pressure plays a signiﬁcant role in the formulation of a modern theory of plasticity. It has been assumed by many researchers that plastic yielding of metals is independent of superimposed hydrostatic pressure and that metals are plastically incompressible. In this section, we examine the experimental ﬁndings that have been reported in the literature so that the validity of the aforementioned assumptions can be assessed. We would like

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

235

(a) 2.5

Stress

2 1.5

s

1 0.5 0.2

0.4

0.6

0.8

1.0

log

(b) 2.5 s

Stress

2 1.5

1 0.5 0.2

0.4

0.6 log

0.8

1.0

FIGURE 5.17 Stress–strain curve expressed in two stress measures, (a) tensile and (b) compression.

to mention that the dependence of the yield stress and the compressibility of material on the hydrostatic pressure are well recognized for such porous materials as geotechnical materials and is not be discussed in this section (see Chapter 9 for discussion). Bridgman published a large volume of papers related to high hydrostatic pressure. The experiments related to the studies of large plastic ﬂow under the effect of hydrostatic pressure are well summarized in Bridgman [9]. From the many solids studied, the “absolute compressibility” of the material is given from [3, p. 493] by −

V = a p − b p2 V0

(5.47)

where p is the hydrostatic pressure measured in kgf/cm2 (1 kgf/cm2 = 98.1 kPa), V the volume change, V0 the initial volume at atmospheric pressure, and a and b are constants determined from experiments, for example, a = 5.826 × 10−7 and b = 0.8 × 10−12 for iron. We note that the absolute compressibility expressed by (5.47) is a volumetric strain and would like to mention a special note by Bell [3, p. 494] that Bridgman measured the change

© 2005 by Chapman & Hall/CRC Press

236

Continuum Mechanics and Plasticity

in length in a single direction from which, assuming isotropy, he computed the change of volume. In the tension of steel under hydrostatic pressure, Bridgman [9, p. 49] measured the change in length of the specimen and by the assumption of volume constancy he determined the area reduction of the neck in the tension specimen. He found that the ﬂow stress and the stress at maximum load increase almost linearly with pressure for pressure up to 2,800 MPa (400,000 psi) for various heat treatment of a steel, Bridgman [9, p. 69–70]. Bridgman [9, p. 195] conducted uniaxial compression test using specimens of various metals to determine plastic volume change. No hydrostatic pressure was applied in this series of tests. He used a dilatometer apparatus for determining the change of volume of the specimen during the test. He argued for the superiority of a direct measurement (by use of dilatometer) of the volume change as compared with its indirect determination from measurements of the change of longitudinal and lateral dimensions. Bridgman considered a cylinder of mild steel plastically shortened to 0.85 its initial length by an axial load of 689 MPa (100 ksi), and he compared the radius of the cylinder under two conditions: assuming no change of volume and assuming the full elastic change of volume corresponding to this stress. He found that the radius in the two cases differs only by 0.07%, which is a difﬁcult task for measurement. Bridgman did not compare the circumferential strain, however. If he did, he would have found that the difference is 0.94%, and the circumferential strains are 0.08465 and 0.08545, respectively, which is not a difﬁcult task for today’s measurement technology. Bridgman immersed the specimen undergoing plastic deformation in a dilatometer, which was ﬁlled with a liquid and provided with a capillary open to the atmosphere in which the liquid meniscus moved in response to changes in volume of the contents of the dilatometer. Of the materials examined under compression, negative plastic volumetric strains were shown by annealed high-carbon steel, 303 stainless steel, copper, and hard-drawn brass, and the opposite effect, a positive plastic volumetric strain, was shown by mild steel and iron. With these differences, the plastic volumetric strains were small, however, and most volume changes were recoverable on release of stress. Examples were: the plastic volumetric strain for 1035 steel was 0.0001 for an axial strain of 0.02; it was 0.00012 for 303 stainless steel for an axial strain of 0.135; and it was 0.00015 for high-carbon steel for an axial strain of 0.14. Crossland [35] and Hu [36] found that the yield stress in torsion was sensitive to the presence of hydrostatic pressure up to 280 MPa (40 ksi). Crossland found that the upper yield stress of mild steel decreased by 10% and Hu found that it decreased by 6.5% over the same range of hydrostatic pressure. Permanent volume expansion was observed for 4310 and 4330 steels by Spitzig et al. [7]. These authors determined the density at the uniform gauge section of the specimen. Measurements were made both before and after straining specimens up to 4% plastic strain, and, therefore, these were permanent volume changes. Additional volume-change measurements were made during deformation on several tension specimens with rosette strain

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

237

gauges. It was found that tensile and compressive testing under hydrostatic pressure up to 1100 MPa (160 ksi) raises the stress–strain curve by about 6.5%, but does not signiﬁcantly affect the work-hardening characteristics. The plastic volumetric strain increased proportionally with the axial strain, and it was about 2 × 10−4 when the axial strain was 0.04. Volume-change measurements made from the strain gauges were similar in magnitude to those obtained from the density measurements. For the hydrostatic pressure of 1400 MPa (200 ksi) the elastic volumetric strain is 8.78×10−3 and the plastic volumetric strain is only 2% of this amount. It may be concluded that the yield stress of metallic materials depends on superimposed hydrostatic pressure. The yield stress in tension, compression, or torsion may increase or decrease with pressure depending on material tested. Further investigation to experimentally quantify this effect is warranted. However, for a ﬁrst approximation, the assumption that plastic yielding of metals is independent of superimposed hydrostatic pressure is reasonable. We are convinced that the plastic volumetric strain is small compared to the elastic volumetric strain. Therefore, the assumption of plastic incompressibility is well established. The assumption of plastic incompressibility is expressed in terms of the increments of the plastic strain as p

p

p

p

dεkk = dε11 + dε22 + dε33 = 0

5.5 5.5.1

(5.48)

Torsion Test in the Large Strain Range Introduction

Torsion tests in the large strain range provide results that are useful in the development and veriﬁcation of microstructure-based and phenomenological constitutive models of crystalline solid. The test is quite complex since, in addition to shear stress and shear strain, the axial and hoop strains and the axial stress are also important, making torsion test a multi-axial test. There are two end-conditions in the torsion test: the ﬁxed-end and the free-end torsion. In the ﬁxed-end torsion, the length change of the specimen is prevented, and, because of this, axial stress is developed during torsion. On the other hand, the length change is permitted in the free-end torsion, but the axial stress is zero during torsion. The existence of axial stress or axial strain in the torsion test is generally known as the axial effect. Some torsion tests are cited as: Poynting [37], Swift [38], Hughes [39], Hodierne [40], Ronay [41,42], Baily et al. [43], Billington [44], Lindholm et al. [45], Van Arsdale et al. [46], Montheillet et al. [47], Wu et al. [2,48], Lipkin and Lowe [49], White et al. [50], Weerasooriya and Swanson [51], Toth et al. [52], and Miller and McDowell [53]. Several problems related to such torsion tests need to be addressed. If these problems are not carefully considered, then the validity of test results may be questioned. The problems are associated with the homogeneity of the

© 2005 by Chapman & Hall/CRC Press

238

Continuum Mechanics and Plasticity

material, the strain measurement, the specimen geometry, and the determination of the shear stress–strain curve from the experimental torque versus angle of twist curve. These problems have been discussed in [2] and the following discussions are based on [2]. (1) The material homogeneity: If the material is not homogeneous, nonuniform deformation will occur, leading to regions that remain almost undeformed while plastic deformation occurs in the remaining part of the specimen. The strain concentration will lead to an early development of shear band localization in the specimen. This is a very serious problem, especially when long gauge-length specimens are used. In the research of [2], well controlled, homogeneous material was supplied by a material manufacturer and macroscopically uniform plastic deformation (no apparent regions of strain concentration were observed by eye inspection after the test) was obtained in all specimens tested. (2) The strain measurement: An important problem associated with the torsion test and the combined axial–torsion test is the strain measurement. A transducer that measures and controls normal and shear strains in the large strain range is not generally available. Almost all experimental results reported in the literature use the relative motion between the grips to compute the axial and shear strains. This method does not lead to accurate strain measurements due to the geometry of the specimen, which has enlarged ends. An axial–torsional extensometer has been designed and built by Wu and Xu [1], see Figure 5.18. This extensometer measures strains in the gauge section of the solid shaft or tubular specimens. Speciﬁcations of the extensometer have been determined in terms of the linearity, cross-talk, and hysteresis, and have been reported in Wu and Xu [1]. In particular, the cross-talk between axial and shear channels is 150◦ C (300◦ F), which is the upper temperature limit for the LVDTs and RVDTs of the extensometer. For higher temperature tests, a different method of calibration must be used and specimens were required in this procedure. Calibration curves were determined at room and 150◦ C temperatures. It was then assumed that these curves were still valid at higher temperatures. A total of four short specimens of cast aluminum were used for the calibration tests in free- and ﬁxed-end torsion conditions. Figure 5.20(c) shows the calibration curves plotting the grips rotation of the test machine against the relative rotation within the gauge length, measured by the extensometer, of a short specimen tested in free-end torsion at two different temperatures. It is seen that no noticeable differences can be found between the two curves. This curve describes the geometrical characteristic of the specimen and shows that the relation has not been affected by temperature. Similar calibration curves for short specimen subjected to ﬁxed-end torsion have also been obtained. Again, temperature does not have a noticeable inﬂuence on the calibration curve. The calibration curves plotting the stroke of the test system versus the axial extension within the gauge length of a specimen have also been determined and it has been found that the curve is not affected by test temperature either. An assumption is then made that these curves remain unchanged at higher temperatures at 205◦ C (400◦ F) and 315◦ C (600◦ F), so that they may be used to convert the stroke and rotation readings recorded during tests at 205◦ C and 315◦ C into axial and shear strains, respectively. At these temperatures, due to an added heating element, about 3 to 4 h of heating time were needed for the environmental chamber to reach a steady uniform temperature. 5.5.2.3 The hoop strain measurement There are rarely any experimental data reported concerning the hoop strain. Baily et al. [43], recorded the hoop strain by taking readings of ﬁnal diameter for nine specimens, which were tested at different levels of shear strain. However, a plug was used during the torsion tests, which might have restricted the diametral change. Although the diameter reduction was observed by many investigators (Swift [38], Freudenthal and Ronay [56], Ronay [41]) no reliably recorded data were taken either during the tests or after the tests. Data of diameter can provide important information as much as the axial extension does. In [2], the hoop strain was determined by accurately measuring the diameter change during torsion. A ring was attached to the middle of the gauge section of the specimen by use of four, equally spaced (90◦ apart), spring-loaded pins. Two pins located at the opposite side of the diameter of the specimen

© 2005 by Chapman & Hall/CRC Press

246

Continuum Mechanics and Plasticity

formed a pair. The displacement of each pin was measured by a LVDT and the readings for each pair of pins were averaged. This data and that obtained from the second pair of pins were then averaged to provide the data for diametral change during torsion. In order to conﬁrm the measured diametral change, a micrometer with 0.0025 mm (0.0001 in.) accuracy was used to measure the diameter. The measurement was taken at upper, middle, and lower cross-sections within the gauge section after each test run at room temperature. Several test runs were conducted, one after the other, so that a shear strain of 200% was obtained. After the tests, the specimens were cut in the middle section and the diameters were again measured. The data were consistent with the LVDT readings. The hoop strain was then computed by dividing the diametral change by the initial diameter. In the tests for measuring the diametral change, the axial and shear strains were determined by the stroke and rotation, respectively, of the test machine. These readings were then converted into axial and shear strains by use of a set of calibration curves, one of which is shown in Figure 5.20(c).

5.5.3

Experimental Results and Discussions

Experimental results of [2] were analyzed and presented in terms of true shear stress–strain curve, axial strain, hoop strain, and axial stress. The difference between the cast and the extruded aluminum and the effect of test temperature are discussed in each item. Finally, the effect of specimen geometry is also discussed. 5.5.3.1 The true shear stress–strain curve Raw experimental data in terms of torque versus angle of twist curves were analyzed by the modiﬁed Nadai method presented by Wu et al. [20]. The method accounts for length change in free-end torsion, and it is a method to determine the true shear stress–strain curve without measurement of radial and hoop strains. The true shear stress is deﬁned in Wu et al. [20,22] based on the current cross-section of the specimen. The method of Wu et al. [20,22] is discussed in Section 5.5.4. The axial strain was computed simply by dividing the axial extension by the initial gauge length. It was a good approximation, since the axial extension was a small deformation. In the case of ﬁxed-end torsion, Nadai’s method [6] was used, since there was no axial length change. Figure 5.21 shows the shear stress–strain curves for extruded aluminum at room and 150◦ C (300◦ F) temperatures. It is seen that the stress is lower at 150◦ C and that the shear stress–strain curve of ﬁxed-end torsion is slightly higher than that for free-end torsion. This difference is due to the analysis (Wu et al. [20]) which assumes that the hoop strain and axial strain ratio is 0.5. According to the experimental results to be presented later in this section, this ratio is much greater than 0.5. An analysis by use of [22] with

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

247

60

Shear Stress (MPa)

50 40 30

Fixed-end (Short) Free-end (Short) Free-end (Long) Fixed-end (Short 300° F) Free-end (Short 300° F)

20 10 0 0

25

50

125 75 100 Shear Strain (%)

150

175

FIGURE 5.21 Shear stress–strain curves for extruded aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

80

Fixed-end (Short) Free-end (Short) Free-end (Long) Free-end (Medium) Room Temperature

Shear Stress (MPa)

60

Fixed-end (Short 300° F) Free-end (Short 300° F)

40 Fixed-end (Short 400° F) Free-end (Short 400° F)

20

Free-end (Short 600° F) Fixed-end (Short 600° F)

0 0

50

100 Shear Strain (%)

150

200

FIGURE 5.22 Shear stress–strain curves for cast aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

the hoop strain and axial strain ratio equal to 0.9 would make the two curves coincide. This correction has been made for curves in Figure 5.22 which are for cast aluminum. It sufﬁces to mention that the curves for ﬁxed-end torsion in Figure 5.21 are the true stress–strain curves.

© 2005 by Chapman & Hall/CRC Press

248

Continuum Mechanics and Plasticity 150

Mises Stress (MPa)

Cast P0815 Aluminum ATC Compression Test

100

Extruded P0815 Aluminum Tabular Specimen Torsion 50

0

Cast P0815 Aluminum Tabular Specimen Torsion

0.0

0.2

0.4 Effective Strain

0.6

0.8

FIGURE 5.23 Comparison of mises stress obtained from torsion and compression (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

The curves of Figure 5.22 were obtained from free- and ﬁxed-end torsion tests at room, 150◦ C (300◦ F), 205◦ C (400◦ F), and 315◦ C (600◦ F) temperatures using long, medium, or short specimens. It is seen that these curves are strongly affected by temperature. The higher the temperature is, the lower is the shear stress–strain curve. Short specimens were tested at all four temperatures. The curves of those specimens under ﬁxed- and free-end condition are indistinguishable at all temperature levels. Long and medium gauge length specimens were also used in the room temperature testing under free-end condition. It is seen that the curves at room temperature for specimens of all gauge lengths are very close to each other. Figure 5.23 shows the experimental data of cast and extruded aluminum from the present torsion tests compared to the compression tests obtained by Wang et al. [57]. Note that there is an interruption in the compression curve due to unloading and specimen remachining. The curves are plotted in the form of Mises stress versus effective strain. (The Mises stress is deﬁned based on the Mises yield criterion, which is discussed in Chapter 6 in connection with the ﬂow theory of plasticity; and the effective strain is deﬁned based on the second invariant of the strain tensor.) It is seen that the torsion curve for extruded aluminum, which has prestrain texture, lies higher than that for cast aluminum. Furthermore, the ﬁgure shows that the mises stress cannot be used to obtain a uniﬁed stress–strain curve for cast aluminum, because the stress for compression test is higher than that for torsion test. This is so because the two tests lead to different textures. 5.5.3.2 The axial strain The axial effect takes the form of length change during free-end torsion. Figure 5.24 summarizes test data for axial extension versus shear strain for

© 2005 by Chapman & Hall/CRC Press

Fundamentals of Continuum Plasticity

249

4 Extruded P0815 Aluminum Long and Short Specimens Axial Strain (%)

3

2

1 Cast P0815 Aluminum (1/8⬙, 1/4⬙ and Solid)

0 0

30

60

90

120

150

Shear Strain (%) FIGURE 5.24 Axial strain in free-end torsion for cast and extruded aluminum (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

cast and extruded aluminum. The effect of specimen geometry is signiﬁcant and is discussed in a subsequent section. For extruded aluminum, the axial extension starts to increase at the early stage of torsion test and continues to increase thereafter. The notation EAL denotes extruded aluminum with long specimen and EAS denotes extruded aluminum with short specimen. The wall-thickness was 6.4 mm for both curves. The slopes of axial strain curves decrease slightly at large shear strain level. For cast aluminum, the rate of axial extension is very small when the shear strain is 50%. In the ﬁgure, CA1/8 denotes cast aluminum tubular specimen with 3.2 mm (1/8 in.) wall-thickness and medium gauge length; CA1/4 denotes cast aluminum tubular specimen with 6.4 mm (1/4 in.) wall-thickness and long gauge length; and CASOL denotes cast aluminum solid shaft specimen. This ﬁgure shows that the development of axial effect in the cast aluminum was delayed by a shear strain of approximately 50% when compared with the extruded aluminum. Figure 5.25 shows that the test temperature does not have a signiﬁcant inﬂuence on the axial extension for cast aluminum. In the case of extruded aluminum (not shown in the ﬁgure), the axial extension curve at room temperature is slightly higher than that at 150◦ C (300◦ F), but they almost coincide. This ﬁnding does not agree with the assertion [41] that a higher temperature would give rise to a larger axial extension, and it is not consistent with the temperature effect observed in the axial stress developed during ﬁxed-end torsion test discussed in the next subsection. Different textures are developed at different test temperatures and they can cause different amounts of length

© 2005 by Chapman & Hall/CRC Press

250

Continuum Mechanics and Plasticity 2.0

300° F (Short)

Axial Strain (%)

1.5

400° F (Short) 600° F (Short)

1.0

0.5

0.0 0

25

50 75 Shear Strain (%)

100

125

FIGURE 5.25 Axial strain in free-end torsion at elevated temperature (From Wu, H.C. et al., Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

change. It is believed that the specimen geometry effect is responsible for this inconsistency. The geometry effect is important in the free-end torsion test and not as important in the ﬁxed-end torsion test. Therefore, it is believed that the observed dependence of the axial stress on temperature is a true effect. From this viewpoint, one can then infer that a temperature effect should also exist in the length change, but it should be further investigated. 5.5.3.3 The hoop strain For a few specimens where the outer diameter change was measured during free-end torsion, the hoop strain was computed from the diametral change. Figure 5.26 shows the axial and hoop strains plotted against the shear strain for cast and extruded aluminum at room temperature. Two long specimens of extruded aluminum (marked “textured” in the ﬁgure) were tested and the results are very consistent. The axial strain was about 5.5–6% and the hoop strain was about 4.0–4.5% when the shear strain was 150%. In the case of cast aluminum (marked “nontextured”), two medium and one short specimen were tested. It is seen that the development of the axial and hoop strains was delayed as compared to the curves of extruded aluminum. In all curves, no noticeable differences can be observed between specimens for shear strain of 150%, the ratio is over 0.9. For the cast specimens, the ratio is hard to determine at shear strain of 0

when f = k 2 and df = 0 (plastic state)

(6.36)

Expression (6.36a) describes the condition when the stress point is either inside the yield surface or is on the yield surface but is about to move inward; (6.36b) describes the condition when the stress point is moving on the yield surface; and (6.36c) describes the condition when the stress point is stationary on the yield surface. We make the following remarks for this model: 1. The increments of plastic strain depend on the current values of deviatoric stress and not on the stress increment. 2. The principal axes of stress and of plastic-strain-increment tensor coincide. The ﬂow rule satisﬁes the experimental ﬁnding that the plastic-strain-increment vector is normal to the yield surface if the Mises yield criterion is used. 3. No plastic volume change during plastic deformation is assumed, p that is, dεii = dλσii = 0. 4. The magnitude of plastic strain increment is determined by dλ, which in turn is determined by the actual increment of plastic work given by p

dW p = σij dεij = dλσij σij = dλ( 13 σkk δij + σij )σij = dλ( 13 σkk σii + σij σij ) = −2 dλ J2 = 2 dλ k 2

(6.37)

From (6.37), we obtain p

dλ =

σij dεij 2k 2

© 2005 by Chapman & Hall/CRC Press

p

=

((1/3)σkk δij + σij )dεij 2k 2

p

=

σij dεij 2k 2

p

=

σij deij 2k 2

(6.38)

278

Continuum Mechanics and Plasticity p

p

p

p

where dεij = 13 δij dεkk + deij = deij . A slightly different form of (6.38) can be found if we consider the following expressions: σij deij

=

σij (deije

p + deij ),

deije

=

dσij 2µ

,

dJ2 = −σij dσij = 0 (−J2 = k 2 = const) and σij deij =

σij dσij 2µ

p

(6.39) p

+ σij deij = σij deij

Using the last expression of (6.39), (6.38) becomes dλ =

σij deij 2k 2

=

σij (dεij − 13 δij dεkk ) 2k 2

=

σij dεij 2k 2

(6.40)

The Prandtl–Reuss equation may then be written as dεij =

dε σij σkm km 1 1 dσkk δij + dσij + 9K 2µ 2k 2

(6.41)

This equation relates dεij to dσij and σij , and it can be written in the form [dεij ] = [Aijkm ][dσkm ]

(6.42)

where Aijkm is a function of σij . Note that this method of determination of dλ works when f is a function of stress only and is in the form of the Mises yield criterion. In the more general expressions for f , dλ may be determined by use of the consistency condition to be discussed later. The class of perfectly plastic material is an idealization with the purpose of keeping the constitutive equation simple. This idealization is reasonable for materials that do not show signiﬁcant strain-hardening. The adequacy of this idealization depends on the purpose and requirement of the speciﬁc application. If only monotonic loading is of interest and it does not call for a reﬁned solution, then this idealization may very well lead to a satisfactory solution with a minimum amount of mathematics. However, due to the progress in industries, which give rise to problems that are subjected to complex loading conditions and impose stricter requirements, this idealization is no longer adequate in many applications. In those cases, reﬁnement of the theory is called for and strain-hardening should be considered. The reﬁnement of the ﬂow theory is discussed in Chapter 7. An example to demonstrate the differences between an elastic material and an elastic-perfectly plastic material is given by a strain-controlled test with proportional strain path as shown in Figure 6.9. Assuming that the experiment begins at point O (Figure 6.9(a)), moves to B , and continues © 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

279

(a)

(b)

C⬘

C B

B⬘ D

O⬘

O

FIGURE 6.9 (a) A proportional strain path and (b) corresponding stress trajectories for elastic (OBC) and elastic-perfectly plastic material (OBD). ,

n B⬘ B(, )

Φ

,

O

FIGURE 6.10 A controlled linear stress path and its corresponding strain path.

on to point C in the strain space. The corresponding trajectories in the stress space shown in Figure 6.9(b) are OBC for elastic material and OBD for elasticperfectly plastic material. It is seen that the two stress paths show drastic differences for the same strain path. It is a nonlinear path for the latter case. Details related to stress- and strain-controlled tests for an elastic-perfectly plastic material are discussed in Examples 6.1 to 6.3. In a stress-controlled combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, if the stress-path OB (Figure 6.10) is linear, ﬁnd the corresponding strain path.

EXAMPLE 6.1

Solution The states of stress and strain are 2 3σ σ τ 0 σij = τ σij = τ 0 0 , 0 0 0 0

τ σ − 3 0

0 0 , σ − 3

ε γ εij = 2 0

γ 2 0 0

0 0 0 (a)

© 2005 by Chapman & Hall/CRC Press

280

Continuum Mechanics and Plasticity

(b)

B

(a)

C C⬘

Φ

B⬘

O⬘

O

FIGURE 6.11 (a) A controlled proportional strain path and (b) the corresponding stress path.

Lateral strains have been neglected due to the smallness of their magnitudes, but they may be considered for better accuracy. In the elastic state from O to B (and also O B in the strain space), the relations are εe =

σ , E

γe =

τ µ

(b)

and the slope of the strain path (Figure 6.11(a)) is deﬁned by tan φ =

µσ µ εe = = tan e γ Eτ E

(c)

where is known. The strain path during the elastic state is denoted by OB’. In the elastic–plastic state, dλ = 0, and the Prandtl–Reuss equation is from (6.41) dεij =

dε σij σkm km 1 1 dσkk δij + dσij + 2 9K 2µ 2k

(d)

Since the test is stress-controlled and follows a straight path, the stress point will remain at B after yielding has occurred. Thus, dσij = 0. Hence, we have dεij =

dε σij σkm km

(e)

2k 2

The nonzero components of (e) are dε =

σ 3k 2

2 σ dε + τ dγ 3

© 2005 by Chapman & Hall/CRC Press

,

dε12 =

τ 3k 2

2 σ dε + τ dγ 3

(f)

The Flow Theory of Plasticity

281

and the strain increment has the following slope after yielding has occurred dε12 3τ = dε 2σ

dγ 3τ = dε σ

or

(g)

We now show that this direction is parallel to the normal to the yield surface at B. This is the direction of the strain path after yielding has occurred at B . The yield surface is f = 12 σij σij − k 2 = 0

(h)

For the stress state of (a), (h) reduces to f = σ 2 + 3τ 2 − 3k 2 = 0

(i)

The gradient of the yield surface is ∂f ∂f ∂σrs ∂f = = ∂σij ∂σrs ∂σij ∂σrs

1 δri δsj − δrs δij 3

=

σrs

1 δri δsj − δrs δij 3

= σij (j)

So, the components of the normal n are proportional to nσ ∝ σ11 = 23 σ ,

nτ ∝ σ12 =τ

(k)

with a slope nτ 3τ = nσ 2σ

(l)

Note that this slope is the same as that of dε12 /dε in (g). It is wrong to differentiate the yield function (i) in the τ –σ subspace to obtain the normal as nσ ∝

∂f = 2σ , ∂σ

nτ ∝

∂f = 6τ , ∂τ

nτ 3τ = nσ σ

(m)

This slope is different from that in (l). The correct way is to make distinction between σ12 and σ21 and differentiate the yield function with respect to σ12 . But, the τ –σ stress space is convenient for engineering application and, in this case, we must work with the engineering shear strain γ instead of the tensorial shear strain ε12 . Therefore, we use the γ –ε strain space, and observe that the slope in this strain space given by the second equation of (g) is the same as the slope in (m).

© 2005 by Chapman & Hall/CRC Press

282

Continuum Mechanics and Plasticity

In a strain-controlled, combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, if the strain-path OB C is linear (Figure 6.11(a)), ﬁnd the corresponding stress path.

EXAMPLE 6.2

Solution The states of stress and strain are given in (a) of Example 6.1 and the elastic phase of the problem is the same as in Example 6.1. In this range, the slope of the strain path is known and is given by m = tan φ =

ε dε µσ = = γ dγ Eτ

(a)

Yielding can occur when the stress reaches B and the strain reaches B . The last relation of (a) is σ−

mE τ =0 µ

(b)

The stresses at B may be determined from the intersection of (b) with the yield locus (6.11). They are σB =

√ 3 mkE 3µ2 + m2 E2

and

τB =

√ 3 kµ 3µ2 + m2 E2

(c)

If yielding would occur at B with a stationary stress point (Figure 6.11(b)), that is, dσij = 0, then using (6.41), the Prandtl–Reuss equation would have components dε = dε p =

σ 3k 2

2 σ dε + τ dγ , 3

dγ = dγ p =

τ k2

2 σ dε + τ dγ (d) 3

and the direction of the plastic strain increment evaluated at B would be dγ 3τB 3µ 1 = =

= dε σB mE m

(e)

We see that the slope of the strain increment in (e) is not the same as the controlled slope 1/m, and, therefore, the stress point cannot be stationary at B, and dλ = 0 at B. The stress point must move away from B in a neutral loading along the yield locus until it reaches point C, where the normal of the yield locus is parallel to the controlled strain slope O B C of Figure 6.11(a). The Prandtl–Reuss equation applies and we set the slope in (e) to 1/m, that is, σ − 3mτ = 0

© 2005 by Chapman & Hall/CRC Press

(f)

The Flow Theory of Plasticity

283

(b)

B, C

(a)

C⬘ B⬘

D⬘ at ∞

O⬘

O

D

FIGURE 6.12 (a) A controlled strain path and (b) the corresponding stress path.

The intersection between this line and the yield locus (6.11) is found at σC =

3 mk 1 + 3m2

τC =

,

k 1 + 3m2

,

with

σC = 3m = 3 tan φ τC

(g)

Thus, the slope of OC is deﬁned by angle θ as θ = tan−1 (3 tan φ)

(h)

The stress point stays at C upon further increase of the strain point beyond C . EXAMPLE 6.3 In a strain-controlled, combined tension–torsion test of a tubular specimen of an elastic-perfectly plastic material, determine the stress-path that corresponds to the strain-path OB C D shown in Figure 6.12(a). Yielding occurs at B .

Solution The elastic state is governed by Hooke’s law. Plastic deformation occurs from B to C , while the stress stays at B. The states of stress and strain during this stage are

0 σij = τ 0

τ 0 0

0 0 , 0

0 σij = τ 0

τ 0 0

0 0 , 0

0

εij = γ 2 0

0

0 0

0

0

γ 2

(a)

The nonzero component of the Prandtl–Reuss equation is dγ =

© 2005 by Chapman & Hall/CRC Press

dτ τ 2 dγ + 2 µ k

(b)

284

Continuum Mechanics and Plasticity

or

τ2 dτ = µ 1 − 2 k

dγ

(c)

But, on the yield locus, using (6.11) and (a), τ 2 = k 2 . Thus, dτ = 0 and C stays at B on the yield locus. Next, we consider the stage from C to D . The strain-path C D has increment in the axial strain only, while the shear strain is kept constant, that is, dγ = 0. Due to the effect of elastic strain, dγ p = 0. Therefore, plastic deformation occurs. The states of stress and strain are the same as that of (a) of Example 6.1. Putting dγ = 0, the shear component of the Prandtl–Reuss equation (6.41) is dτ = −

2σ τ µ dε + 3τ 2

(d)

σ2

Substituting (d) into the differential form of yield function (6.11), we obtain dσ =

6τ 2 µ dε σ 2 + 3τ 2

(e)

It is easy to show that the stress increment (dτ , dσ ) is tangential to the yield locus. This is not a neutral loading, however, because the plastic strain is taking place. The plastic strain increments are found from (6.41) as dεp =

2 σ 2 dε 9 k2

and

dγ p =

2 σ τ dε 3 k2

with dγ = 0

(f)

By use of (d) and (e), both dτ and dσ may be calculated for a given dε. These equations may be integrated to obtain a closed form solution. From (d) and (6.11), we have 2µτ k 2 − τ 2 dτ = − dε √ 3 k2

or

τ

dτ k2

− τ2

2µdε = −√ 3 k2

(g)

This equation may be integrated to obtain √ 3k 1 − 1 − (τ/k)2 ε= ln 2 µ τ/k

(h)

where, by use of the boundary condition that τ = k when ε = 0, the integration constant is zero. Introducing now nondimensional variables X = µε/k

© 2005 by Chapman & Hall/CRC Press

Nondimensional Stresses

The Flow Theory of Plasticity 1

285

Z

0.8 0.6 0.4 Y 0.2 0

2 4 6 8 Nondimensional Axial Strain, X

10

FIGURE 6.13 Nondimensional shear (Y) and axial (Z) stresses as axial strain increases.

for strain and Y = τ/k for stress, (h) may be solved for Y to yield Y=

√ 3 √ 1 + e(4X)/ 3

2e(2X)/

(i)

Figure 6.13 shows the plot of Y versus X. It is seen that the shear stress gradually reduces as the axial strain increases. Similarly, (e) may be integrated to yield √

σ −1 + e(4X)/ 3 √ Z= √ = 3k 1 + e(4X)/ 3

(j)

Z may be plotted against X and the relationship is also shown in Figure 6.13. Using (i) and (j), X may be eliminated to obtain Y 2 + Z2 = 1

(k)

which is the yield locus (6.11). Thus, the stress point moves, generating plastic deformation, along the yield locus and end up in D as shown in Figure 6.12(b). √ Deﬁne an equivalent (effective) stress as σ¯ = 3/2{σij σij }1/2 √ and an equivalent (effective) plastic strain increment as d¯ε p = 2/3× p p p {dεij dεij }1/2 , show that the plastic work increment is dW p = σij dεij = σ¯ d¯ε p . EXAMPLE 6.4

Solution From (6.37), we have p

dW p = σij dεij = 2dλ k 2

© 2005 by Chapman & Hall/CRC Press

(a)

286

Continuum Mechanics and Plasticity

Using (6.32), (6.34), and (a), the equivalent plastic strain increment is

2 p p 1/2 dεij dεij = d¯ε = 3 2 dλ 2 dW p =√ k = √ 3 k 3k

p

2 1/2 dλ σij σij = 3

√ 2 dλ( 2k) 3 (b)

Thus, dW p =

√ 3k d¯εp

(c)

On the other hand, the equivalent stress is σ¯ =

3 1/2 = σ σ 2 ij ij

√ 3 √ ( 2k) = 3k 2

(d)

Combining (c) and (d), we obtain p

dW p = σij dεij = σ¯ d¯εp

(e)

Note that equivalent (or effective) quantities such as the equivalent (or effective) stress, the equivalent (or effective) strain, or the equivalent (or effective) strain rate are often used in dealing with the multidimensional behavior of isotropic materials. This equivalent quantity often represents the magnitude of that quantity.

6.5

Strain-Hardening

There are three classes of materials: the strain-hardening material, the perfectlyplastic material, and the strain-softening material. Generally, metals are strainhardening (or work-hardening) materials and geotechnical materials may exhibit strain-softening under certain conditions. Several criteria have been proposed to classify the materials. Generally, the strain-hardening material is regarded as a stable material. Drucker [21] proposed to classify materials by the now well-known Drucker’s postulate, which is not a law of thermodynamics, but a means of classiﬁcation. Materials obeying Drucker’s postulate can then be studied by a theory of plasticity that can be built up based on that postulate. In the multiaxial stress state, strain-hardening is considered in the form of hardening rules for subsequent yield surfaces. Experimental determination of subsequent yield surfaces is discussed in Chapter 7. It has been observed that the yield surface, upon application of a deformation history, will undergo expansion, distortion, translation, and rotation. A precise description of these

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

287

characteristics is deferred to Chapter 12. In this section, we discuss a simpliﬁed version of the hardening rules and consider only the expansion (isotropic hardening) and translation (kinematic hardening) of the yield surface. This simpliﬁed version has been widely used in the mechanics literature. 6.5.1

Drucker’s Postulate

Drucker’s postulate consists of two parts: the stability in the small and the stability in the large. These are described by the following statements: 1. The stability in the small: The work done by an external agency, which slowly applies an additional set of forces to the already stressed material, over the displacement it produces, is positive. 2. The stability in the large: The net work performed by the external agency over the cycle of application and removal is positive, if plastic deformation has occurred in the cycle. The aforementioned external agency is entirely separate and distinct from the agency that causes the existing state of stress and that has produced the existing state of strain. The cycle of application is the stress cycle and is different from Ilyushin’s strain cycle, which is not as restrictive as the stress cycle. The meaning of the above statements are now explained. In the one-dimensional case, let us consider Figure 6.14(a). The stress at A is already the existed state. The stability in the small says that an external agency increases the stress from A to C and the work done represented by area ACE is positive; the stability in the large says that the work done by the external agency over the stress cycle of σ ∗ to σA and then to σC and then back down to σ ∗ and represented by area BACDB is positive. σ ∗ is an arbitrary stress state in the elastic region. In the multidimensional case, we consider a stress cycle described in Figure 6.14(b). At time t = 0, the stress point is at B and denoted by σij∗ , which is an arbitrary point within or on the current yield surface, so that p

f (σij∗ , εij , κ) ≤ 0 (a)

*

A

(b)

C E

t1, ij

B t = 0, ij* tf, D

B D

FIGURE 6.14 Stress cycles: (a) one-dimensional and (b) multiaxial.

© 2005 by Chapman & Hall/CRC Press

A

(6.43)

C + d , t ij ij 2

p

p

f (ij +dij, ij +dij , + d ) = 0 p

f (ij, ij , ) = 0

288

Continuum Mechanics and Plasticity

where κ is a strain-hardening parameter. The yield function is expressed in terms of stress σij , which is possible as in (6.12) or (6.13). Furthermore, for strain-hardening materials, the yield function f depends on the prestraining p history and we include the plastic strain εij and a parameter κ in the yield function for generality. At point A (t = t1 ), the stress point σij is on the yield surface so that p

f (σij∗ , εij , κ) = 0

(6.44)

The stress point then pierces the yield surface and carries the yield surface with it, until at point C, where t2 = t1 +dt, it reaches the dashed curve which is governed by p

p

f (σij + dσij , εij + dεij , κ + dκ) = 0

(6.45)

Additional plastic deformation has occurred during this step. Unloading then follows, which brings the stress point back to σij∗ at B. The corresponding time is t = tf . At this point, p

p

f (σij∗ , εij + dεij , κ + dκ) ≤ 0

(6.46)

The work done during this stress cycle is W=

0

tf

(σij − σij∗ )˙εij dt =

t2

t1

p

(σij − σij∗ )˙εij dt ≥ 0

(6.47)

The last expression has accounted for the fact that the work done by the elastic strain dεije for a closed path is zero. In this stress cycle, the plastic deformation only occurs in the step AC. We now take Taylor series expansion of the above integral about t = t1 as p p p W (t2 ) = (σij − σij∗ )˙εij t=t dt + 12 [σ˙ ij ε˙ ij + (σij − σij∗ )¨εij ]t1 (dt)2 + · · · ≥ 0 1

(6.48) with W (t1 ) = 0. For the stability in the small, σij∗ and σij coincide at t1 , and the above expression is reduced to p

W = 12 σ˙ ij ε˙ ij (dt)2 + · · · ≥ 0

(6.49)

Take the time increment dt small enough that the higher order terms in dt are negligible, we obtain p

σ˙ ij ε˙ ij ≥ 0

or

p

dσij dεij ≥ 0

which is the expression for the stability in the small.

© 2005 by Chapman & Hall/CRC Press

(6.50)

The Flow Theory of Plasticity

289

In the case of σij∗ = σij at t1 , by neglecting the second and higher order terms, we have from (6.48) p

W = (σij − σij∗ ) ε˙ ij dt ≥ 0

p

(σij − σij∗ ) dεij ≥ 0

or

(6.51)

This is the expression for the stability in the large. By the use of Drucker’s postulate, it is possible to show that the yield surface is convex and that the plastic strain increment is normal to the yield surface. Without the use of this postulate, these two effects would have been two separate assumptions. We discuss the case that the yield surface is smooth without corners. Let σij be any regular point on the yield surface and σij∗ p be an arbitrary point inside or on the yield surface. Let dεij be the plastic p strain increment at σij . Then, (6.51) shows that the vectors (σij − σij∗ ) and dεij are making an acute angle and that the arbitrary σij∗ must lie on the side p

p

of the hyperplane opposite to that from which dεij is directed. dεij is normal to the hyperplane as shown in Figure 6.15(a). Since σij is a regular point of the yield surface, the hyperplane must be tangent to the yield surface, and, p therefore, dεij is normal to the yield surface at the point of tangency σij . This also establishes the convexity of the yield surface at point σij . p Next, we show that the direction of dεij is independent of the direction of (σij − σij∗ ) if the yield surface is regular. Assuming that two different (σij − σij∗ ) p give rise to two different dεij . Then, the yield surface f1 = 0, which is perp(1) pendicular to dεij must intersect with the yield surface f2 = 0, which is p(2) perpendicular to dεij at an angle (see Figure 6.15(b)). Thus, the yield surface is nonregular at σij , which contradicts with the assumption that it be p regular at σij . Therefore, the two dεij ’s must not be different and the direction p of dεij is independent of the direction of (σij − σij∗ ). In the case when f = 0 is nonregular at σij , the normality condition cannot be p established. Drucker’s postulate only requires that dεij lie within a bounded angle at a pointed vertex of the yield surface. However, nonregular yield

(a)

(b)

p

dij

p(1)

dij

p(2)

dij

Hyperplane p normal to dij ij ij*

FIGURE 6.15 Normality of plastic strain increment.

© 2005 by Chapman & Hall/CRC Press

=0

f1

f2

=0

290

Continuum Mechanics and Plasticity

surfaces have not been experimentally observed as mentioned in Section 6.2. Therefore, this case will not be pursued.

6.5.2

The Isotropic-Hardening Rule

We call a strain-hardening an isotropic hardening, if the subsequent yield surface is an isotropic expansion of the initial yield surface as shown in Figure 6.16(a). The Bauschinger effect is not considered in the isotropic hardening. The yield function is expressed by f (σij ) = Y 2

(6.52)

where Y is the yield stress under uniaxial tension. Y represents the radius of the yield surface and, when it increases, the yield surface expands in size. Y can be a function of either one of the two quantities that are used to measure the degree of hardening: the plastic work per unit volume deﬁned by Wp =

p

σij dεij

(6.53)

or the equivalent plastic strain with increment deﬁned by p

d¯ε =

2 p p 1/2 dεij dεij 3

(6.54)

An equivalent stress deﬁned by σ¯ =

(a)

3 1/2 σ σ 2 ij ij

(6.55)

(b)

ur

fa c

e

q Su bse

t uen

rfa

ce

S

Su

I n i t i a l Yi el d

l Yie

d

FIGURE 6.16 (a) Isotropic hardening and (b) schematic equivalent stress–plastic strain curve.

© 2005 by Chapman & Hall/CRC Press

p

The Flow Theory of Plasticity

291

is usually introduced to describe the isotropic hardening. The equivalent stress can also take the following forms σ¯ = =

1 2 2 2 1/2 (σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 + 6σ12 + 6σ23 + 6σ31 2 1/2 1 (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 2

(6.56)

The equivalent√stress is deﬁned based on the Mises yield criterion (6.6), √ observing Y = 3 k. Equation (6.6) reduces to Y = (3/2){σij σij }1/2 , which is of the same form as (6.55). Thus, σ¯ = Y and we write either Y = σ¯ = F(W p )

(6.57)

or

d¯εp

Y = σ¯ = H

(6.58)

where F and H are functions and these functions are to be determined by plotting experimental stress–strain curves in the form of σ¯ versus ε¯ p as shown in Figure 6.16(b). There are efforts to obtain a universal stress–strain curve, such as (6.57) or (6.58), which encompasses all states of stress [22]. Using this concept, a shear stress–strain curve can be deduced from a tensile stress–strain curve. We invert the function of (6.58) to obtain

d¯εp = H −1 (σ¯ ) or

ˆ σ¯ )dσ¯ d¯ε p = F(

(6.59)

where the function H is known from experiment. Using the ﬂow rule (6.35), the equivalent plastic strain increment is from (6.54) p

d¯ε =

2 2 1/2 = dλ σij σij 3

2 2 2 dλ σ¯ = dλσ¯ 3 3 3

(6.60)

Equating (6.59) and (6.60), we ﬁnd dλ =

3 F(σ¯ )dσ¯ 2

where F(σ¯ ) =

ˆ σ¯ ) F( σ¯

(6.61)

Therefore, the ﬂow rule is written as p

dεij = 32 F(σ¯ )dσ¯ σij

© 2005 by Chapman & Hall/CRC Press

(6.62)

292

Continuum Mechanics and Plasticity

In the case of uniaxial tension, (6.62) reduces to p

dε p = dε11 = 32 F(σ¯ )dσ¯ ( 23 σ ) = F(σ¯ )dσ¯ σ

(6.63)

and, in the case of pure torsion in a thin tube, (6.62) is p 1 2 dγ

p

= dε12 = 32 F(σ¯ )dσ¯ τ

(6.64)

The expression of equivalent stress for uniaxial tension is σ¯ =

3 1/2 {σ σ } = 2 ij ij

2 σ 2 1/2 3 2 =σ σ +2 − 2 3 3

(6.65)

and for pure torsion is σ¯ =

3 1/2 = σ σ 2 ij ij

√ 3 {2τ 2 }1/2 = 3 τ 2

(6.66)

Thus, we ﬁnd σ τ=√ 3

(6.67)

Substituting (6.67) into (6.63) and (6.64), we obtain dγ p =

√ 3 dεp

(6.68)

We now use (6.67) and (6.68) to deduce a shear stress–strain curve (τ , γ ) from a known tensile stress–strain curve (σ , ε). In a monotonic loading condition, (6.68) is integrated to yield γp =

√ p 3ε

or

(γ − γ e ) =

√ 3(ε − ε e )

or

γ−

√ τ σ = 3 ε− µ E (6.69)

Using (6.67) and the relations of elastic constants, (6.69) reduces to γ √ =ε− 3

1 − 2ν 3E

σ

(6.70)

where ν is Poisson’s ratio. Knowing (σ , ε) for any point on the tensile curve, we can use (6.67) and (6.70) to determine the corresponding point (τ , γ ) on the shear curve. We can also use a graphical method to accomplish the task. Referring to Figure 6.17, we need to establish ﬁrst, the two elastic lines with slopes E and µ. At point A on the tensile line, the stress is σA . Segment AB is the

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

293

corresponding plastic strain ε p , which is known. Next, locate point C on the √ elastic shear line with stress equals to σ / 3. The length of line segment CD A √ is 3 εp and, therefore, point D can be located. The process may be repeated for all points to determine the shear stress–strain curve. In the case of combined axial–torsion of a thin-walled tube, if we use the Mises yield function and isotropic hardening, the ﬂow rule is given by (6.62). (a) Determine the function F(σ¯ ) from a uniaxial tension test. (b) For the general case of combined tension and torsion, ﬁnd the expressions for the axial and shear strain increments. (c) For a stress-controlled proportional stress-path OBC shown in Figure 6.18, ﬁnd the corresponding strain path. (d) For a stress-controlled torsion from O to Afollowed by tension ABCD while

EXAMPLE 6.5

le Tensi

A

B(, )

A C A

Shear

D(, )

E

3

AB = p CD = 3 p

FIGURE 6.17 Determination of shear stress–strain curve from the tension stress–strain curve.

, D⬘

n B⬘

C B (, )

Φ

n

fC fB

,

O FIGURE 6.18 Stress-controlled proportional stress path assuming isotropic hardening.

© 2005 by Chapman & Hall/CRC Press

294

Continuum Mechanics and Plasticity dp

B

A

C

O

D

FIGURE 6.19 A torsion–tension stress path assuming isotropic hardening.

keeping the shear stress constant at τA (Figure 6.19), discuss the corresponding strain path. Solution For a combined axial–torsion test, the states of stress and strain are 2 γ σ τ 0 3 0 ε σ τ 0 γ 2 σ σij = τ 0 0 , σij = τ εij = − 0 , 0 0 3 2 0 0 0 σ 0 0 0 0 0 − 3 (a) The equivalent stress and its increment are from (6.55) and (a) σ¯ = {σ 2 + 3τ 2 }1/2 ,

dσ¯ =

σ dσ + 3τ dτ σ¯

In the case of uniaxial tension, the Prandtl–Reuss equation is dσ 3 2 dε = dε11 = + F(σ¯ )dσ¯ σ E 2 3

(b)

(c)

and the equivalent stress and its increment are σ¯ = σ ,

dσ¯ =

σ dσ σ¯

(d)

Using (d), (c) may be written as dε 1 F(σ¯ )σ 2 1 = = + dσ Et E σ¯

© 2005 by Chapman & Hall/CRC Press

(e)

The Flow Theory of Plasticity

295

where Et is the slope of the tensile stress–strain curve. Solving (e), we ﬁnd F(σ¯ ) =

1 σ¯

1 1 − Et E

(f)

For the general case of combined tension and torsion, by use of the ﬂow rule (6.62) and the elastic strains, the two components of the Prandtl–Reuss equation are

1 1 − (σ dσ + 3τ dτ ) Et E dτ 1 3τ 1 dγ = + (σ dσ + 3τ dτ ) − µ E (σ¯ )2 Et σ dσ + dε = E (σ¯ )2

(g)

For the stress-controlled proportional stress-path OBC shown in Figure 6.18, the elastic state OB is the same as that of Example 6.1 and shown previously in Figure 6.10 with angle φ. At point B of Figure 6.18, yielding ﬁrst occurs with corresponding yield locus fB . The normal to the yield locus is denoted by n. As the stress path proceeds from B to C, the stress point carries the yield locus with it and the yield locus makes an isotropic expansion. The normal to the yield locus fC at C is still n. Taking the plastic strain part of (g), we obtain the following ratio for the plastic strain increments 3τ dγ p = p dε σ

(h)

It is easily shown that this slope is normal to the yield locus. However, the strain-path B D is not in the same direction as the normal n because of the elastic strain. Path B D has to be determined by integrating (g). We now discuss a stress-controlled torsion from O to A followed by tension ABCD while keeping the shear stress constant at τA (Figure 6.19). During the stage of tensile loading ABCD, the strain increments are given by (g) with dτ = 0. Thus, dσ 1 1 σ2 dε = − + (dσ ) E E (σ¯ )2 Et 3τA σ 1 1 dγ = − (dσ ) E (σ¯ )2 Et

(i)

We see from (i) that the plastic strain ratio is 3τA dγ p = = tan ϕ p dε σ

(j)

The angle ϕ of the plastic strain vector changes from 90◦ at A to smaller angles as the axial stress σ increases. As σ becomes large, the angle ϕ tends

© 2005 by Chapman & Hall/CRC Press

296

Continuum Mechanics and Plasticity

to zero. We note that this result is merely a prediction of the model with isotropic hardening. Related experimental results are discussed in Chapter 7. The plastic-strain-increment vectors are shown in Figure 6.19. Finally, we mention that the strain path is found by integrating the expression (k) which is obtained by eliminating dσ from (i) dγ [3τA σ/(σ¯ )2 ][(1/Et ) − (1/E)] = dε 1/E + (σ 2 /(σ¯ )2 )[(1/Et ) − (1/E)]

6.5.3

(k)

The Kinematic-Hardening Rule

The kinematic-hardening rule assumes that the yield surface translates without rotation in the stress space. The shape and size of yield surface remain unchanged during motion of yield surface. This hardening rule has been introduced by Prager [23] to account for Bauschinger effect. Hodge [24] pointed out that the concept of kinematic hardening must be applied in the nine-dimensional stress space. In the nine-dimensional space, the initial yield surface is given by f (σij ) = 0

(6.71)

and the subsequent yield surface by f (σij − αij ) = 0

(6.72)

where αij is the total translation of center of initial yield surface and is termed back stress by some investigators. Note that for Mises criterion, we write

σij − αijD σij − αijD = 2k 2

(6.73)

where αijD is the deviatoric part of αij . Hodge [24] further suggested the concept of combined isotropic–kinematic hardening. In this case, the yield surface translates, deﬁned by αij , and expands as well, which is deﬁned by the change in k. The evolution rule of αij in the stress space is of interest. Prager [23] proposed a linear-hardening rule as p

dαij = c dεij

(6.74)

where c is a constant. Ziegler [25] proposed a modiﬁed kinematic-hardening rule as dαij = dµ(σij − αij )

© 2005 by Chapman & Hall/CRC Press

where dµ > 0

(6.75)

The Flow Theory of Plasticity

297

The directions of dαij are different between (6.74) and (6.75) and they are shown in Figure 6.20. In (6.75), dµ is a parameter and should not be mixed with the shear modulus. In the ﬁgure, O is the origin of the nine-dimensional stress space and O is the center of the current yield surface. The current stress point is at P. According to (6.74), the center of yield surface would translate in a direction normal to the yield surface at P and this increment of (P) translation is denoted by dαij in the ﬁgure. On the other hand, according (Z) to (6.75), the increment of translation of the yield surface, denoted by dαij , is along the direction of O P. We note that the two rules are the same if the current yield surface is a hypersphere, which is true when the Mises yield surface is considered and a combined isotropic–kinematic hardening is applied. The linear kinematic hardening can only be applied to a material with a bilinear stress–strain curve when unloading and reverse loading is considered. For a nonlinear stress–strain curve, the linear kinematic-hardening rule would result in an unloading curve, which bends in an unnatural way and such an unloading curve has never been observed. Figure 6.21(a) shows such (p)

dij

(z)

dij

O⬘

P

ij

ij f=0

O

ij

FIGURE 6.20 Kinematic-hardening rules by Prager and Ziegler.

(a)

(b) rve d cu Loa

Y

h

O

h

ss k stre Bac

cu load Un

rve

p

h

FIGURE 6.21 Linear kinematic-hardening: (a) nonlinear stress–strain curve and (b) bilinear stress–strain curve.

© 2005 by Chapman & Hall/CRC Press

298

Continuum Mechanics and Plasticity

a behavior in the one-dimensional loading–unloading stress–strain curve. The linear kinematic hardening rule, applied to a bilinear stress–strain curve (a special case of (6.58)), is shown in Figure 6.21(b), where the stress σ is plotted against the plastic strain ε p . In the ﬁgure, Y is the initial yield stress and the slope of the linear kinematic hardening is h, that is, dα = h dεp

(6.76)

In the case of uniaxial loading, the increment of the back stress is

dα dαij = 0 0

0 0 0

0 0 0

and

2 3 dα dαijD = 0 0

0 −

dα 3 0

−

0 0 dα

(6.77)

3

Thus, from (6.74), the ﬁrst element of the linear kinematic hardening rule is 2 3 dα

= c dεp

(6.78)

Comparing (6.76) with (6.78), we obtain h = 32 c

(6.79)

and the stress–stress curve during loading is given by σ = Y + h εp

(6.80)

Thus, h is also the slope of the stress–strain curve. In case of nonlinear loading curve, the yield function is f (σij − αij ) = Y 2

(6.81)

in which both Y and αij are not constant for combined isotropic–kinematic hardening. The increment of stress in the uniaxial stress σ versus plastic strain ε p plot consists of two parts, that is, dσ = dY + dα

(6.82)

Introduce an isotropic–kinematic-hardening parameter β, which is a number 0 ≤ β ≤ 1. Then, we may write dY = βh dεp

© 2005 by Chapman & Hall/CRC Press

and

dα = (1 − β)h dε p

(6.83)

The Flow Theory of Plasticity

299

and (6.82) becomes dσ = h dε p

(6.84)

The extreme value β = 1 characterizes isotropic hardening and β = 1 characterizes kinematic hardening. When β has a value between 0 and 1, then we have a case of combined isotropic–kinematic hardening. The combined isotropic-linear kinematic-hardening rule cannot lead to a reasonable unloading curve. Nonlinear kinematic-hardening rules will have to be used to describe the unloading curve. A nonlinear kinematic-hardening rule was ﬁrst used by Armstrong and Frederick [26] and written as p

dαij = 23 c dεij − καij d¯ε p

(6.85)

where c and κ are material constants. This rule has gained popularity in recent literatures. We will see in Chapter 8 that this hardening rule is also a part of the endochronic theory of plasticity proposed by Valanis [27] and was applied by Wu and Yang [28] and Wu et al. [29]. Denoting the increment of equivalent plastic strain by the increment of a monotonically increasing positive parameter z, so that dz = |d¯ε p |

(6.86)

then (6.85) may be written as p

dαij 2c dεij + καij = dz 3 dz

(6.87)

If c and κ are constants, then (6.87) is a linear ordinary differential equation with constant coefﬁcients and the solution is 2c αij (z) = 3

p

z

e

−κ(z−z )

z0

dεij (z ) dz

dz + αij (0) e−κ(z−z0 )

(6.88)

In (6.88), z is the current value of the parameter; z0 is the initial value of z; and αij (0) is the initial value of αij (z). In the case of uniaxial loading–unloading, (6.90) reduces to α(z) =

2c 3

z

z0

e−κ(z−z )

dε p (z ) dz + α(0) e−κ(z−z0 ) dz

(6.89)

Referring to Figure 6.22, let us consider loading along OA and then unloading to B. The initial conditions are z0 = 0 and α(0) = 0. We note that

© 2005 by Chapman & Hall/CRC Press

300

Continuum Mechanics and Plasticity A

Normalized Back Stress

0.4 0.3 0.2 B

0.1

O

0.01

0.02 0.03 Strain p

0.04

0.05

FIGURE 6.22 Loading–unloading curves for nonlinear kinematic-hardening.

[dε p (z )/dz ] = +1 during loading, and [dε p (z )/dz ] = −1 during unloading. Using these conditions, (6.89) may be integrated during loading to yield y = 1 − e−κz = 1 − e−κε

p

with y =

3κ α 2c

(6.90)

where y is a normalized back stress. Unloading occurs at point A and (6.89) is integrated to obtain the unloading curve as α(z) =

2c 3

0

zA

e−κ(zA −z ) (+1) dz +

= α(zA ) +

2c 3

z

zA

2c 3

z

zA

e−κ(z−z ) (−1) dz =

e−κ(z−z ) (−1) dz + α(0)e−κ(z−z0 ) 2c 2c [1 − e−κzA ] − [1 − e−κ(z−zA ) ] 3κ 3κ

2c −κzA −κ(z−2zA ) = [e − 1] e 3κ

(6.91)

The value of z at A is denoted by zA . Referring to (6.86), during loading, we have dz = d¯εp = dεp ; but during unloading, when z > zA , we have dz = −dεp . This relation may be integrated starting from point A to obtain ε = εA + zA − z = 2zA − z

(6.92)

Substituting (6.92) into (6.91), we obtain p

y = e−κεA [eκε − 1] p

(6.93)

Equations (6.90) and (6.93) are plotted in Figure 6.22. We see that the curves for loading and unloading do not coincide and they are curved. The slopes for loading and unloading curves starting at any point such as A are different. © 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

301

The differential form (6.85) for the uniaxial loading–unloading is dα = c dε p − κα d¯ε p = (c − κα)dε p = (c + κα)dε

for loading

p

for unloading

(6.94)

where (6.94) deﬁnes the slopes for the two cases. Finally, we mention that the linear kinematic-hardening rule leads to a straight line applicable to both loading and unloading. 6.5.4

General Form of Subsequent Yield Function and its Flow Rule

In order to have a more general description of yield surface, let us consider p that the yield function is a function of stress σij , plastic strain εij , and a parameter κ, and write p

f (σij · εij , κ) = 0

or

p

f (σij · εij , κ1 ) = κ0 = const

(6.95)

where κ0 represents the size of the yield surface. Referring to Figure 6.23, p points A and B have the same εij and κ0 , and, without κ1 , we are not able p to distinguish A from B. We have to know dεij and dκ1 to determine the subsequent yield surface. The ﬂow rule is from (6.32) p

dεij = dλ

∂f ∂σij

(6.32)

On the other hand, Drucker’s postulate gives p

dσij dεij = dλ dσij

∂f >0 ∂σij

(6.96)

where (∂f /∂σij )dσij > 0 represents the loading condition. Comparing the above two expressions we found dλ > 0. A

O

B

FIGURE 6.23 Parameters for yield surface.

© 2005 by Chapman & Hall/CRC Press

302

Continuum Mechanics and Plasticity

The parameter dλ is determined by use of the consistency condition, Prager [30]. Since loading from a plastic state must again lead to a plastic state, the stress and plastic strain that exist after the inﬁnitesimal changes p dσij , dεij , and dκ have taken place must still satisfy (6.97), which is p

f (σij , εij , κ) = 0

(6.97)

By use of the consistency condition, the increment of the yield function is zero, that is, df =

∂f ∂f ∂f p + dκ = 0 dσij + p dεij + ∂σij ∂κ ∂εij (A)

In Figure 6.24, the stress at point A is σij

(6.98)

and it is on the yield surface

(A) p(A) f σij , εij , κ (A) = 0

(6.99)

An inﬁnitesimal loading has moved the stress point from A to B and it carries (B) the yield surface with it, so that the stress at B is σij and the yield surface that B is on is (B) p(B) f σij , εij , κ (B) = 0

(6.100)

(B) p(A) f σij , εij , κ (A) > 0

(6.101)

while

Substituting (6.32) into (6.98), we have df =

∂f ∂f ∂f ∂f dσij + dλ p + dκ = 0 ∂σij ∂κ ∂εij ∂σij

(B)

Β, ij

(A)

A, ij

FIGURE 6.24 The consistency condition.

© 2005 by Chapman & Hall/CRC Press

(6.102)

The Flow Theory of Plasticity

303

which may be solved to obtain dλ as dλ = −

(∂f /∂κ)dκ + (∂f /∂σij )dσij

(6.103)

p

(∂f /∂σrs )(∂f /∂εrs )

Therefore, by use of (6.32), the ﬂow rule is p

dεij =

(∂f /∂κ)(∂f /∂σij )dκ + (∂f /∂σkm )(∂f /∂σij )dσkm p

−[(∂f /∂σrs )(∂f /∂εrs ]

(6.104)

Note that this equation consists of two parts. One part is due to dκ and the other part is due to dσij ; but the stress increments appear in the scalar form involving summation. p The increment dκ may be assumed to be a linear function of dεij , such that p

p

p

p

dκ = hrs (σmn , εmn )dεrs = h11 dε11 + h12 dε12 + · · ·

(6.105)

Then, dκ = hkm dλ

∂f ∂σkm

(6.106)

By use of (6.106), (6.102) reduces to ∂f ∂f ∂f ∂f ∂f df = =0 dσij + dλ + hkm p ∂σij ∂κ ∂σkm ∂εij ∂σij

(6.107)

We then solve (6.107) for dλ to obtain dλ =

−(∂f /∂σij )dσij p

(∂f /∂σrs )(∂f /∂εrs ) + (∂f /∂κ)(∂f /∂σrs )hrs

(6.108)

Therefore, (∂f /∂σkm )(∂f /∂σij )dσkm

p

dεij =

p

−[(∂f /∂σrs )(∂f /∂εrs ) + (∂f /∂κ)(∂f /∂σrs )hrs ]

(6.109)

p

This equation shows that dεij is linearly related to dσkm and (6.109) is in the following form p

p

dεij = Aijkm (σrs , εrs , κ)dσkm

© 2005 by Chapman & Hall/CRC Press

(6.110)

304

Continuum Mechanics and Plasticity

We have thus shown that the linear relation of (6.110) between the plastic strain and stress increments follows from the normality condition of plastic strain-rate by assuming a linear relationship for dκ given by (6.105). A special case of (6.110) is, Hill [16, p. 33], p

dεij = Gij

∂f dσkm ∂σkm

(6.111)

where Gij is a symmetric function of stress and strain history, but is not a function of dσkm . In addition, Gii = 0. Equation (6.111) has been applied in [16] to the case of isotropic hardening. If we choose ∂g ∂σij

(6.112)

∂g ∂f dσkm ∂σij ∂σkm

(6.113)

Gij = h then, (6.111) becomes p

dεij = h

in which h = h( J2 , J3 ) and g = g( J2 , J3 ) is the plastic potential. We see that (6.113) is in the form of (6.109). Another special case of (6.112) is p

dεij = G

∂f ∂f dσkm ∂σij ∂σkm

(6.114)

This form was used by Drucker [31]. In the equation, G is any positive scalar function of stress, strain, and history κ, but is independent of dσkm . An important special case is the kinematic hardening. Consider the yield function f (σij − αij ) = 0

(6.115)

in the stress space. Let pij = σij − αij , then ∂f ∂pij ∂f ∂f ∂f = = δik δjm = ∂σkm ∂pij ∂σkm ∂pij ∂pkm ∂f ∂f ∂pij ∂f = =− ∂αkm ∂pij ∂αkm ∂pkm

(6.116)

Thus, ∂f ∂f =− ∂σij ∂αij

© 2005 by Chapman & Hall/CRC Press

(6.117)

The Flow Theory of Plasticity

305

Using the yield function (6.115), the consistency condition is df =

∂f ∂f dσij + dαij = 0 ∂σij ∂αij

(6.118)

Using (6.117), we then have ∂f ∂f dσij − dαij = 0 ∂σij ∂σij

(6.119)

If we apply Prager’s linear-hardening rule, we obtain ∂f ∂f p dσij − c dεij = 0 ∂σij ∂σij

(6.120)

∂f ∂f ∂f dσij − c dλ =0 ∂σij ∂σij ∂σij

(6.121)

or

Hence, (∂f /∂σkm )dσkm c[(∂f /∂σij )(∂f /∂σij )]

(6.122)

(∂f /∂σij )(∂f /∂σkm )dσkm c[(∂f /∂σij )(∂f /∂σij )]

(6.123)

dλ = and the ﬂow rule is p

dεij =

This equation may also be derived from (6.106) by setting dκ = 0. Equation (6.104) becomes p

dεij =

(∂f /∂σij )(∂f /∂σkm )dσkm p

−[(∂f /∂σrs )(∂f /∂εrs )] p

(6.124) p

In this case, the yield function is given by f (σij , εij ) = 0, where σij and εij are treated as independent variables. By use of Prager’s linear-hardening rule, we write ∂f p ∂εrs

=

∂f ∂f c=− c ∂αrs ∂σrs

(6.125)

Combining (6.124) and (6.125), we obtain (6.123). If we use Ziegler’s kinematic-hardening rule, then dαij = dµ(σij − αij )

© 2005 by Chapman & Hall/CRC Press

with dµ > 0

(6.126)

306

Continuum Mechanics and Plasticity

The consistency condition is ∂f ∂f dσij − dµ (σij − αij ) = 0 ∂σij ∂σij

(6.127)

dµ =

(∂f /∂σij )dσij (σkm − αkm )(∂f /∂σkm )

(6.128)

dαij =

(∂f /∂σrs )dσrs (σij − αij ) (σkm − αkm )(∂f /∂σkm )

(6.129)

df = Therefore, we obtain

and

p

We see that the evolution of αij is not directly related to dεij . But, the ﬂow rule for this case is still given by (6.32), in which dλ cannot be determined from the consistency condition. Instead, dλ is determined from the normality condition as follows: we deﬁne a plastic modulus K along the direction of the outward normal n at the stress point on the yield surface. The stress increment projected along n is dσ = n · dσ and the following relation holds: (n · dσ)n = K dεp

with K > 0

(6.130)

Therefore, the ﬂow rule is dεp =

6.6

1 dσ (n · dσ)n = n K K

(6.131)

The Return-Mapping Algorithm

We discussed in Section 6.5.4 how the plasticity factor dλ can be determined by means of the consistency condition of Prager [30]. This method has been applied extensively in the literature to solve boundary-valued problems of plastic deformation involving simple states of stress. For multidimensional engineering problems of plasticity, a numerical algorithm has been developed, which is known as the return-mapping algorithm (or the backward Euler integration algorithm). For constitutive equations in the rate form, the numerical procedure calls for the determination of quantities at step (n + 1) using information at step (n). The return-mapping algorithm assures that the incremental step from (n) to (n + 1) is consistent with the ﬂow rule and hardening rule, and the stress point at step (n + 1) is lying on the subsequent yield surface. Referring to Figure 6.25, the current stress σ (n) is at A and the stress at the next step σ (n+1) is at B. The task is to determine the stress at point B

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

307 C, T(n + 1) F

A, (n)

E

B, (n + 1) D ∆e

∆ p ∆ E

FIGURE 6.25 The return-mapping algorithm in one-dimensional stress.

for a strain increment ε. Starting from A, point C is the trial step known as the elastic predictor, its stress denoted by σ T(n+1) . DC is obtained by multiplying the total strain increment ε by the elastic modulus E. From the ﬁgure, we see that AE is the plastic strain increment ε p and ED is the elastic strain increment εe . BC is equal to EF, which is obtained by multiplying εp by the elastic modulus E. BC is known as the plastic corrector. The stress increment DB = elastic predictor − plastic corrector = DC − BC. In the multidimensional case, the algorithm is formulated below: The elastic predictor is T(n+1)

σij

(n)

(n+1)

= σij + Cijkm εkm p(n+1)

and the plastic corrector is Cijkm εkm (n+1)

σij

T(n+1)

= σij

p(n+1)

− Cijkm εkm

(6.132)

, so that the stress at step (n + 1) is

(n)

(n+1)

= σij + Cijkm εkm

p(n+1)

− Cijkm εkm

(6.133) Similar procedure should be applied to other variables of the model, such as the back stress to account for the evolution of that variable. Figure 6.26 illustrates this algorithm in the multidimensional stress space. Let the yield surface at step (n) be (n) f σij , κ (n) = 0

© 2005 by Chapman & Hall/CRC Press

(6.134)

308

Continuum Mechanics and Plasticity T(n + 1)

(n+1)

Plastic Corrector

(n)

f ((n + 1)) = 0

f ((n)) = 0

FIGURE 6.26 The return-mapping algorithm in the multidimensional stress space. (n)

(n+1)

so that σij is on the yield surface. If σij

is inside the surface, such that

(n+1) (n) f σij ,κ 0 ,κ f σij

(6.136)

then, the return-mapping algorithm ensures that it is lying on the yield surface corresponding to step (n + 1), that is, (n+1) (n+1) f σij ,κ =0

(6.137)

In this case, dλ > 0, which can be determined by substituting (6.133) and the ﬂow rule into (6.137) and solving the resulting equation for dλ. Additional information about the return-mapping algorithm may be found in Simo and Hughes [32]. It sufﬁces to mention that, for associative plasticity with convex yield surfaces, the plastic corrector phase of the algorithm has the unique property that it yields the so-called closest point projection.

6.7

Combined Axial–Torsion of Strain-Hardening Materials

We consider a thin-walled tube made of strain-hardening metal. The coordinate system is chosen so that the radial direction is denoted by 1, the hoop

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

309

direction is 2, and the axial direction is 3. The Mises yield criterion will be used together with three cases of strain-hardening rule: the isotropic hardening, the kinematic hardening, and the combined isotropic–kinematic hardening. We will ﬁrst derive the equations for axial tension and pure torsion, and then present, in Example 6.6, the case in which the tube is ﬁrst subjected to torsion into the plastic range and then subjected to tension while holding the shear stress constant. This problem will be referred to as the tor–ten stress path in this book. We would like to ﬁnd and compare the plastic strains developed due to this loading history using different strain-hardening rules. The yield function is f = ξijD ξijD − 2k 2 = 0

with ξijD = σij − αijD

(6.138)

where shear yield stress which is related to the tensile yield stress by √k is the D Y = 3k. αij is the deviatoric part of back stress αij and ξijD is the deviatoric part of ξij . Using the isotropic–kinematic-hardening parameter β introduced in (6.83), the isotropic-hardening rule is dY = βh d¯ε p

(6.139)

where d¯εp is the equivalent plastic strain increment deﬁned by (6.60). The linear kinematic-hardening rule is p

dαijD = 23 (1 − β)h dεij

(6.140)

and the ﬂow rule is p

dεij = dλ ξijD

(6.141)

In the uniaxial tension, the deviatoric stress, plastic strain increment, and the deviator of the back stress are −σ 3 [σ ] = 0 0 −α

3 [α D ] = 0 0

0 −σ 3 0 0 −α 3

© 2005 by Chapman & Hall/CRC Press

0

0

0 , 2σ 3

−dεp 2 [dεp ] = 0 0

0 −dε p 2 0

0 , 0 dε p

0

0 2α 3

(6.142)

310

Continuum Mechanics and Plasticity

Substituting (6.142) into (6.138), we obtain σ =Y+α

(6.143)

In the case of uniaxial tension, we have from (6.60) and (6.142) 1/2 2 −dε p 2 p 2 (dε ) + 2 = dε p d¯ε = 3 2 p

(6.144)

Thus, dY = βh dεp

(6.145)

Using (6.140) and (6.142), the 33 component equation is 2 3 dα

= 23 (1 − β)h dε p

(6.146)

Therefore, dα = (1 − β)h dεp

(6.147)

Substituting (6.145) and (6.147) into the differential of (6.143), we obtain dσ = h dεp

(6.148)

This equation describes the tensile stress–strain curve for a linear-hardening material independent of the hardening rule. In the torsion of the tube, the deviatoric stress, plastic strain increment, and the deviator of the back stress are

0 [σ ] = 0 0

0 0 τ

0 τ , 0

0

0 [dεp ] = 0

0 0 dγ p 2

0

dγ p 2 , 0

0 [α D ] = 0 0

0 0 α

0 α 0

(6.149) Using (6.149), the yield function reduces to τ =k+α

(6.150)

dγ p d¯εp = √ 3

(6.151)

From (6.60) we have

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

311

and the isotropic-hardening rule is from (6.139) dγ p dY = βh √ 3

or

dk =

βh p dγ 3

(6.152)

The 23 component equation of (6.140) is now dα = 13 (1 − β)h dγ p

(6.153)

The differential form of (6.150) is then obtained as dτ = 13 h dγ p

(6.154)

This equation √ describes the shear stress–strain√curve. We note that if the shear stress is 3τ and the shear strain is dγ p / 3, then (6.154) and (6.148) have the same slope h. Study the tor–ten stress path using the Mises yield criterion with hardening rules given by β = 1, 0, and 0.5.

EXAMPLE 6.6

Solution We use the return-mapping algorithm in this calculation and consider a hypothetical material with shear modulus µ = 26.2 GPa and the initial shear yield stress k = 6.35 MPa. In all three cases, that is, β = 1, 0, and 0.5, we obtain the same shear stress–strain curve shown in Figure 6.27. The slope of the tensile stress–strain curve is assumed to be h = µ/40. The ﬁrst phase of the tor–ten path is in pure torsion and the phase ends when the shear strain γ = 0.01 and the corresponding shear stress τ is 8.47 MPa. At this point, denoted by A in Figure 6.28(a) to (c), the current shear yield stress k is 8.46 MPa for β = 1, 6.35 MPa for β = 0, and 7.41 MPa for β = 0.5; the

Shear Stress , (MPa)

12 10 8 6 4 2 0.005

0.01

0.015

Shear Strain FIGURE 6.27 The shear stress–strain curve for Example 6.5.

© 2005 by Chapman & Hall/CRC Press

0.02

312

Continuum Mechanics and Plasticity

equivalent plastic strain ε¯ p is 0.0056 for all three cases; and the shear back stress α23 is 0 for β = 1, 2.13 MPa for β = 0, and 1.47 MPa for β = 0.5. During the second face of the stress path, AB, the shear stress is kept constant at σ23 = 8.47 MPa, while the axial strain ε increases. The corresponding axial stress σ33 will increase as ε increases. Point B in Figure 6.28(a) to (c) corresponds to ε = 0.012. The quantities σ33 , α33 , α22 , α23 , k, ε¯ p , and γ need to be updated, and dγ p and dε p need to be calculated at each step. Several points along stress-path AB have been chosen for study. The corresponding

(a)

3 23 MPa 30

20

p

dij B

A 10

O a

(b)

(c)

3 23 MPa 30

20

10 b

33 MPa

30

c d e

f

3 23 MPa 30

20 20 A 10 a

p

dij

p

dij b

cd

10

A

e f g B h 20

O

B 10

30 33 MPa

O

ab 10

efg h cd 20

30 33 MPa

FIGURE 6.28 Tor–ten path showing evolutions of yield locus and direction of plastic strain increment for three hardening rules: (a) β = 1, (b) β = 0, and (c) β = 0.5.

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

313

TABLE 6.1 Yield Loci and Direction Angles of Plastic Strain Increments β=1 Yield locus fb fc fd fe ff fg fh

β=0

ε

θ (◦ )

0 0.001 0.005 0.01 0.012

90 37.5 32.9 28.5 26.9

β = 0.5

ε

θ (◦ )

ε

θ (◦ )

0 0.001 0.0025 0.005 0.0075 0.01 0.012

90 58.3 47.7 36.9 30.0 24.8 22.0

0 0.001 0.0025 0.005 0.0075 0.01 0.012

90 61.4 51.1 43.3 37.2 32.7 29.5

yield loci fa , fb , fc , etc. passing through these points are shown in the ﬁgures and are denoted by a, b, c, etc. The yield loci denoted by letter a are the initial yield loci in all three cases. Yield loci with corresponding ε values are listed in Table 6.1. It is clear from Figure 6.28(a) that the yield locus expands centering at the origin O for isotropic hardening. In the case of kinematic hardening, shown in Figure 6.28(b), the yield locus keeps the original size but moves while the tor–ten stress path is pursued. Figure 6.28(c) shows a case of combined isotropic–kinematic hardening with β = 0.5. In this case, the yield locus both expands and moves. The short inclined lines in the ﬁgures show √ p the directions of dεij with components ((dγ p / 3), dεp ). An angle √ p 180 −1 dγ / 3 θ= tan π dε p p

(a)

which is the inclined angle of dεij is deﬁned. At the beginning of the stress path at A, θ = 90◦ for all three cases. In the case of β = 1, θ decreases to 37.5◦ at ε = 0.001 and continues to decrease as ε increases and θ = 26.9◦ at point B. In the case of β = 0, θ decreases to 58.3◦ at ε = 0.001 and continues to decrease as ε increases and θ = 22.0◦ at point B. In the case of β = 0.5, θ decreases to 61.4◦ at ε = 0.001 and continues to decrease as ε increases and θ = 29.5◦ at point B. These angles are listed in Table 6.1. In all cases the directions are normal to the corresponding yield loci. It is evident that different hardening rules lead to different plastic strains. Figure 6.29 plots σ33 versus ε during the stress-path AB. It is seen that the three cases of strain-hardening lead to very different stresses. Isotropic hardening (β = 1) leads to the highest stress of the three cases. This effect can also been seen directly from Figure 6.28(a). The strain paths corresponding to stress-path AB are shown in Figure 6.30. The case of β = 0.5 leads to the highest shear strain. We know that the shear strain has started from the prestrain value of 0.01 during this tension phase. But, the increase in the shear

© 2005 by Chapman & Hall/CRC Press

314

Continuum Mechanics and Plasticity

Axial Stress, (MPa)

30

=1

25 20

= 0.5

15

=0

10 5

0.002 0.004 0.006 0.008 Axial Strain

0.01 0.012

FIGURE 6.29 Axial stresses for tor–ten path.

Shear strain

0.03

= 0.5

0.025 =0 0.02 =1

0.015

0.002 0.004 0.006 0.008 Axial strain

0.01 0.012

FIGURE 6.30 Strain paths for tor–ten path.

strain is still larger than the increase in the tensile strain for cases involving kinematic hardening and the increase is about the same as the increase in the axial strain for the isotropic-hardening case.

6.8

Flow Theory in the Strain Space

The ﬂow theory of plasticity previously presented has been formulated in the stress space. The state of stress is represented by a point in this space and is sometimes referred to as the stress point. If this stress point is located within the yield surface, the material is in the elastic state; and if the stress point is on the yield surface, the material is in the plastic state. The yield surface is deﬁned by a function of stress and other parameters, and the yield surface can expand, distort, or move in the stress space. When the material is in its plastic state, plastic ﬂow occurs according to a ﬂow rule, which deﬁnes the direction and magnitude of the plastic strain increment. Therefore, in this formulation, the stress is the independent variable and the plastic strain

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

315

B A

C D

E

O

FIGURE 6.31 Stress–strain curve of a strain-softening material.

rate (or increment) is the dependent variable. This formulation of plasticity works well for metals and generally works well for strain-hardening materials deﬁned in Drucker’s sense, see Section 6.5. Some materials, such as geotechnical materials (soils, concretes, rocks, ice, etc.) are strain-softening materials. The axial stress–strain curve for this type of materials has a positive slope initially. But, after it reaches a peak, the slope turns into negative. In the region of negative slope, plastic deformation continues with decreasing stress. Figure 6.31 shows a schematic stress–strain curve of a strain-softening material. The stability of strain-softening materials is deﬁned by an Ilyushin postulate [33], which states that the work done by external forces on a material over a closed cycle of strain is positive. In this postulate, work is done over a cycle of strain rather than a cycle of stress as is in Drucker’s postulate. Drucker’s postulate is more restrictive than Ilyushin’s postulate. Referring to Figure 6.31, Drucker’s postulate says that area ABCDA is positive, but Ilyushin’s postulate says that area ABCEA is positive. Ilyushin used strain as an independent variable and stress was a response. He proposed a yield function in the strain space [34] but much of his effort was related to characterizing the stress response to a predetermined strain path. Ilyushin’s work is further discussed in Chapter 7. A ﬂow theory of plasticity expressed in the strain space was proposed by Naghdi and Trapp [35]. Casey and Naghdi [36] further showed that the stress space formulation is a special case of the strain space formulation. In the strain space formulation, the stress response is given by the constitutive equation p

σij = σij (εrs , εrs , κ)

(6.155) p

where κ is the work-hardening parameter. At ﬁxed values of εij and κ, p (6.155) may be inverted to obtain εij as a function of σij , εij , and κ. The yield function (or loading function) in the strain space is p

g(εij , εij , κ) = 0

© 2005 by Chapman & Hall/CRC Press

(6.156)

316

Continuum Mechanics and Plasticity

which corresponds to yield function p

f (σij , εij , κ) = 0

(6.157)

in the stress space. The ﬂow rule is p

ε˙ ij = λρij

∂g ε˙ rs , ∂εrs

if g = 0

and

∂g ε˙ rs > 0 ∂εrs

(6.158)

where λ and ρij are, respectively, a positive scalar-valued function and a p nonzero symmetric tensor-valued function of εij , εij , and κ. If the evolution of κ is p

κ˙ = βij ε˙ ij

(6.159)

then, by use of the consistency condition, it may be shown that (∂f /∂σij )σ˙ ij ∂f ∂g = 1 − λξ (∂g/∂εrs )˙εrs ∂σij ∂εij

(6.160)

p

where ξ is a nonnegative function of εij , εij , and κ. It is seen from (6.160) that the loading conditions in the two spaces are not equal during loading. However, they are equal during unloading and neutral loading. Extensive experimental work has been carried out to determine yield surfaces in the stress space, which is discussed in Chapter 7. Little has been reported concerning experimental determination of yield surfaces in the strain space. But, according to Naghdi and his coworkers [35,36], the yield surface in the stress space can be transformed into the strain space.

6.9

Remarks

We have presented in this chapter the fundamental concept of the ﬂow theory of plasticity. All main elements of the theory have been presented in their simplest forms. We have considered no distortion of the yield surface and the associated ﬂow rule (with normality condition) is used in its simplest form. The isotropic hardening, the kinematic hardening, and the combined isotropic–kinematic hardening have been discussed together with a nonlinear rule of kinematic hardening. In a simplest multiaxial case, the case of combined axial–torsion presented in Section 6.7, we compare results of this simple ﬂow theory using three hardening rules. We have shown that, using this simple model, all three hardening rules lead to the same results for uniaxial tension and pure torsion, but the results for combined axial–torsion vary greatly with the hardening rule assumed. The ultimate question is how

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

317

valid these results are. They show a wide range of differences, and apparently only one of them, or maybe none of them, are correct. In order to establish the validity of a model, the results need to be veriﬁed by experimental ﬁndings. It is the purpose of Chapter 7 to discuss experiments aiming at providing experimental facts that can be used to verify, improve, and reﬁne the theory of plasticity. We will discuss some recently formulated theories and also discuss ideas that extend the theory of plasticity into the ﬁnite strain range.

References 1. Taylor, G.I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc. A. 230, 323, 1931. 2. Bertsch, P.K. and Findley, W.N., An experimental study of subsequent yield surfaces-corners, normality, Bauschinger effect and allied effects, Proc. 4th U.S. Natl. Cong. Appl. Mech., 893, 1962. 3. Mair, W.M. and Pugh, H.L.D., Effect of prestrain on yield surfaces in copper, J. Mech. Eng. Sci., 6, 150, 1964. 4. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Struct., 8, 463, 1972. 5. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 6. Wu, H.C. and Ho, C.C., Strain-hardening of annealed 304 stainless steel by creep, J. Eng. Mat. Tech., 115, 345, 1993. 7. Ishikawa, H., Subsequent yield surface probed from its current center, Int. J. Plasticity, 13, 533, 1997. 8. Szczepinski, W., On the effect of plastic deformation on yield criterion, Arch. Mech., 15, 276, 1963. 9. Batdorf, S.B. and Budiansky, B.A., A mathematical theory of plasticity based on the concept of slip, NACA, TN 1871, 1949. 10. Lin, T.H., A proposed theory of plasticity based on slips, Proc. Second U.S. Natl. Congress Appl. Mech., 461, 1954. 11. Lin, T.H., On stress–strain relations based on slips, Proc. Third U.S. Natl. Congress Appl. Mech., 581, 1958. 12. Phillips, A., A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity, 2, 315, 1986. 13. Mises, R. von, Mechanik der Fasten Korper im plastisch defomablen Zustand, Göttingen Nachrichten, Math. Phys. Kl., 581, 1913. 14. Tresca, H., On the ﬂow of solid bodies subjected to high pressure, C.R. Acad. Sci. Paris, 59, 754, 1864. 15. Lode, W., Versuche über den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle, Eisen, Kupfer und Nickel, Z. Phys., 36, 913, 1926. 16. Hill, R., The Mathematical Theory of Plasticity, Clarendon Press, Oxford, 1950, 38. 17. Hundy, B.B. and Green, A.P., A determination of plastic stress–strain relations, J. Mech. Phys. Solids, 3, 16, 1954. 18. Lianis, G. and Ford, H., An experimental investigation of the yield criterion and the stress–strain law, J. Mech. Phys. Solids, 5, 215, 1957.

© 2005 by Chapman & Hall/CRC Press

318

Continuum Mechanics and Plasticity

19. Phillips, A. and Moon, H., An experimental investigation concerning yield surfaces and loading surfaces, Acta Mech., 27, 91, 1977. 20. Ohashi, Y., Kawashima, K., and Yokochi, T., Anisotropy due to plastic deformation of initially isotropic mild steel and its analytical formulation, J. Mech. Phys. Solids, 23, 277, 1975. 21. Drucker, D.C., A more fundamental approach to plastic stress–strain relations, in Proc. 1st U.S. Natl. Congress Appl. Mech., ASME 487, 1951. 22. Bell, J.F., The experimental foundations of solid mechanics, Handbuch der Physik, Via/1, Flügge, Ed., Springer, Berlin, 1973. 23. Prager, W., The theory of plasticity: a survey of recent achievements ( James Clayton Lecture), Proc. Inst. Mech. Eng., 169, 41, 1955. 24. Hodge, Jr., P.G., Piecewise linear plasticity, Proc. 9th Int. Congress. Appl. Mech., 8, 65, 1957. 25. Ziegler, H., A modiﬁcation of Prager’s hardening rule, Quart. Appl. Math., 17, 55, 1959. 26. Armstrong, P.J. and Frederick, C.O., A mathematical representation of the multiaxial Bauschinger effect, G.E.G.B. Report RD/B/N 731, Berceley Nuclear Laboratories, 1966. 27. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 28. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 29. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 30. Prager, W., Recent developments in the mathematical theory of plasticity, J. Appl. Phys., 20, 235, 1949. 31. Drucker, D.C., A deﬁnition of stable inelastic material, J. Appl. Mech., 26, 101, 1959. 32. Simo, J.C. and Hughes, T.J.R., Computational Inelasticity, Springer-Verlag, New York, 1998. 33. Ilyushin, A.A., On the postulate of plasticity, PMM, 25, 503, 1961. 34. Ilyushin, A.A., Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 196, 1963. 35. Naghdi, P.M. and Trapp, J.A., The signiﬁcance of formulating plasticity theory with reference to loading surfaces in strain space, Int. J. Eng. Sci., 13, 785, 1975. 36. Casey, J. and Naghdi, P.M., On the nonequivalence of the stress space and strain space formulations of plasticity theory, J. Appl. Mech., 50, 350, 1983.

Problems (1) Acylindrical specimen is loaded in tension from 0 to a stress of 500 MPa and has undergone a strain of 0.2 at this point. This point is denoted by A in Figure 6.32. Unloading then occurs following a curve as shown in the ﬁgure. Determine the yield point during unloading, if yield is deﬁned by a proof strain of (a) 0.1%, (b) 0.5%, or (c) 1.0%. Assuming that the yield surface remains circular after prestrain in the two-dimensional principal stress space, sketch the yield

© 2005 by Chapman & Hall/CRC Press

The Flow Theory of Plasticity

319 Stress MPa

A

500 400 300 200 100 0.18

Strain

0.17

0.19

0.20

–100 –200 FIGURE 6.32 Figure for Problem 1.

T L

S

S

A

u

P FIGURE 6.33 Figure for Problem 2.

surfaces corresponding this state of stress using the yield stresses previously determined based on different amounts of proof strain. (2) Consider the three-bar truss shown in Figure 6.33. All bars have the same cross-sectional area A0 and are made of an elastic-perfectly plastic material. Due to the application of force P, the displacement at A is u downward. Assume that the deformation is small so that u/L 1. Determine displacement u, the stresses σT and σS in bars T and S, respectively, and the corresponding strains εT and εS , expressed in terms of p = P/A0 . Plot the p versus u/L diagram. (Hint: Consider the elastic phase, the end of the elastic phase when the ﬁrst bar yields, the elastic–plastic phase, and the end of this second phase.)

© 2005 by Chapman & Hall/CRC Press

320

Continuum Mechanics and Plasticity

(a)

(b) B

A E

O

O

C

D FIGURE 6.34 Figure for Problem 3.

(3) Figure 6.34(a) shows a sketch of uniaxial loading–unloading–reloading curve. Assume that the material obeys Mises yield criterion with kinematic hardening. Sketch in Figure 6.34(b) the yield surfaces that correspond to the stress states of A, B, C, D, and E. Figure 6.34(b) describes the shear versus axial stress space in the combined axial–torsion of a thin-walled tube. (4) A long cylindrical pressure vessel is made of a metal with shear yield stress of k = 560 MPa and the maximum internal pressure during use is limited to 35 MPa. Considering the middle section of the vessel away from the ends, if no section of the vessel is to yield according to the Mises yield criterion, determine the required wall thickness if the outer radius is 600 mm. (5) A closed-ended thin-walled tube is subjected to an axial tensile force F, which is less than F0 necessary to cause yielding. Apply a gradually increasing internal pressure p and determine p expressed in terms of F when yielding occurs. Use Mises yield criterion and denote the wall thickness by t and the mean radius of the tube by r. (6) A metal of yield stress Y = 300 MPa is subjected to a principal stress state of (σ1 , σ2 = −0.2σ1 , σ3 = 0.5σ1 ). If the stress ratios remain constant as the stresses increase, determine σ1 at yielding using the Mises yield criterion. (7) Derive (6.12). (8) Derive (6.13). (9) In a biaxial tension–compression test of perfectly-plastic material, (a) sketch the Mises yield locus, if Y = 250 MPa; ﬁnd the components of the plastic strain increment at the loading point speciﬁed by (b) σx = 250 MPa and σy = 250 MPa; and (c) σx = −100 MPa and σy = 184.52 MPa. √ (10) Find the expression of equivalent stress σ¯ = 3/2{σij σij }1/2 in the case of uniaxial stress. (11) Find the expression of equivalent plastic strain increment d¯εp 2 {dε p dε p }1/2 in the case of uniaxial tension. ij ij 3

© 2005 by Chapman & Hall/CRC Press

=

The Flow Theory of Plasticity

321

(12) What is the deﬁnition of a convex function? p

(13) If the yield function is f = f (σij − c(κ1 )εij ) = κ0 , where κ0 = constant and p

p

κ˙ 1 = (˙εkm ε˙ km )1/2 , assume that the normality condition holds, show that the ﬂow rule is −(∂f /∂σkm )(∂f /∂σij )dσkm

p

dεij =

p

(∂f /∂σrs )(∂f /∂εrs ) + [(∂f /∂σrs )(∂f /∂σrs )]1/2 (∂f /∂κ1 )

(14) Using the equations of Problem (13), show that for Mises’s yield criterion, the ﬂow rule is p

dεij =

(∂f /∂σkm )(∂f /∂σij )dσkm p 2cκ0 + 2κ0 (∂c/∂κ1 )εrs (∂f /∂σrs )

(15) In the case of uniaxial stress, show that the ﬂow rule of Problem (14) reduces to dσ = Et dεp . Determine the expression of Et .

© 2005 by Chapman & Hall/CRC Press

7 Advances in Plasticity

7.1

Introduction

We discussed the basic concepts and formulation of plasticity in Chapter 6. With this knowledge we are ready to explore what other possibilities are there to improve the theory of plasticity. In fact, a great deal of work has been done since 1950 aiming to observe and understand plastic deformation and the mechanics of it. More realistic constitutive models have been proposed. While signiﬁcant progress has been made, still more research work is desirable if the constitutive modeling of plastic deformation is to keep pace with the ever advancing technologies, methods, and equipment of computation. We are currently in a situation where high-powered computational mechanics is using concepts of plasticity that are basic and unsophisticated. The requirement for accuracy of the simulated results will go hand-in-hand with the requirements for safety, efﬁciency, and cost reduction such as reducing the wastes of manufacturing, as various related industries advance. The sophistication of constitutive modeling holds the key to this accuracy requirement. We would like to emphasize that the task of improving the constitutive modeling depends signiﬁcantly on experimental ﬁndings. The experiments will guide the development of theories and theoretical investigation will in turn suggest new experimental conditions. In this chapter, we attempt to describe the state of the art in terms of the experiments which are carried out to improve constitutive modeling. In the theoretical developments, two approaches have been taken by researchers: the traditional plasticity approach with its improvements and a plastic strain trajectory approach, in which the stress depends on the plastic strain trajectory. The traditional plasticity approach is stress-controlled. The stress is the input and the strain is the response. In this approach, we propose a yield function in the stress-space, a ﬂow rule which is usually related to the stress and/or stress increment, and a strain-hardening rule with the back stress moving in the stress space. We discuss in this chapter some modern works belonging to this group. In the plastic strain trajectory approach, the plastic strain path is the input and the stress is found as a response. The relationship between the plastic strain trajectory and the stress is established 323

© 2005 by Chapman & Hall/CRC Press

324

Continuum Mechanics and Plasticity

through a functional or a modulus, depending on whether the constitutive equation is in an integral form or in a differential form. The two forms are equivalent if the boundary conditions are speciﬁed. This approach, including the endochronic theory of plasticity by Valanis [1,2], is brieﬂy described in this chapter. The endochronic theory, which has been derived from the thermomechanical theory of internal state variables, is fully discussed in Chapter 8. We discuss in this chapter how a constitutive equation may be extended to the ﬁnite deformation range. The concept of material objectivity discussed in Chapter 4 must be applied. Appropriate stress and strain measures and their rates should be used. Finally, material texture will develop as plastic deformation proceeds, resulting in material anisotropy. How can the change of material texture be described at the phenomenological level? We attempt to provide research results which address the aforementioned questions.

7.2

Experimenal Determination of Yield Surfaces

The ﬂow theory of plasticity is built upon the concept of yield surface, and therefore yield surface is by far the most important element of all the elements of the theory. We have already discounted Tresca’s yield criterion in the Chapter 6 and concentrated on the Mises yield criterion. But how valid is the Mises yield criterion? Generally speaking, it is a good approximation for initial yield surface (see Section 6.2), although some deviations, such as those shown by Ohashi and Tokuda [3], have been reported. The evolution of the yield surface is of interest to many researchers. As was mentioned in Section 6.2, the size and shape of subsequent yield surfaces depend greatly on the deﬁnition of yield. The yield Surface C of Figure 6.3 determined by the method of backward extrapolation encloses a large elastic region which lies outside of Surfaces B and A. If we insist that the region inside the yield surface is elastic, then the strain is elastic at any point in this region if Surface C is considered as the yield surface. But the same point is outside Surfaces B and A, and therefore, referring to Surfaces B and A, plastic deformation would occur. Apparently, plastic strain is being neglected if Surface C is considered as the yield surface. The quest for more accurate descriptions of the plastic behavior calls for a proportional limit (or small proof strain) deﬁnition of yield, and the challenge is to determine how the yield surface evolves when the material is subjected to various loading histories. These experiments determine the yield function and the back stress which is the center of the yield surface. These are two pieces of information that are central to the ﬂow theory of plasticity. The study of evolution of yield surface has led to the improvements of the theory of plasticity. The effect of various deﬁnitions of yield on the size and shape of subsequent yield surfaces has been previously mentioned. Other factors that affect the determination of yield surface have been discussed by Wu and Yeh [4] and these factors are discussed next (following [4], with permission from Elsevier). © 2005 by Chapman & Hall/CRC Press

Advances in Plasticity 7.2.1

325

Factors Affecting the Determination of Yield Surface

Due to the availability of closed-loop, servo-controlled hydraulic testing machines with sophisticated computer-controlled circuits, it is even more appropriate than ever to discuss some of the factors affecting the determination of yield surface. In earlier test machines, either deadweight or mechanical, “experience” of the investigator was often an important factor in obtaining “reasonable” yield surfaces. With the use of a closed-loop test machine, the “experience” of an investigator can apply only before the beginning of a test or after a test has been completed and no in-between adjustment can be made during the test to smooth out the data. Therefore, it is likely that more data scatter is observed when a closed-loop machine is used, see Phillips and Lu [5]. These data represent more closely the experimental results in their raw form. The deﬁnition of yield by means of a 5µ equivalent plastic strain has gained popularity in the recent literature. One of the reasons for the popularity is that the deﬁnition of yield of 5µ is close to that based on the proportional limit and, therefore, one specimen may be used to determine the initial and all of the subsequent yield surfaces. Astrain of 5µ is, however, a very small strain measured by resistance strain gauges, and there are factors that affect the experiment and may cause a variation of several microstrains. Thus, 5µ is a very sensitive deﬁnition of yield and the resulting data scatter is to be expected. Even though the yield point is based on a proof strain of 5µ, it must be mentioned that the actual plastic strain incurred before a yield point can be conﬁrmed is approximately 10µ. This amount depends on the technical details used by the investigator. The factors presented in the following subsections should be considered in connection with the determination of yield surfaces.

7.2.1.1 The elastic modulus and the zero offset strain For an accurate determination of plastic strain, the “zero offset strain” as shown in Figure 7.1(a) and denoted by ε R should be accounted for. In the ﬁgure, the circular dots represent acquired data for a one-dimensional stress–strain curve and the straight line is an approximation determined by the least mean-square method, using some selected data in the elastic region. Accordingly, the axial plastic strain, ε p , can be determined by εp = ε − ε R −

σ E

(7.1)

where ε is the axial strain; σ is the axial stress; E is Young’s modulus, which is the slope of the straight line, and εR the zero offset strain. The quantity ε R is measured by intersecting the straight line with the ε-axis and is therefore related to the value of E. Ideally, εR should be zero. However, due to the nature of the servo-controlled machine and the time interval of data acquisition, the data will scatter somewhat (exaggerated to show the effect) as shown in Figure 7.1(a). Therefore, some amount of ε R is bound to be present. © 2005 by Chapman & Hall/CRC Press

326

Continuum Mechanics and Plasticity (a)

(b)

P

Y B D

A R

∆p

/E

O

(c)

R

100 c

Shear Stress (MPa)

80

60

d

a

p e

40

20 o 0

b 10 20 30 40 50 60 Axial Stress (MPa)

FIGURE 7.1 (a) Zero offset strain, (b) strain domain Dε , (c) effect of probing path (From Wu, H.C. and Yeh, W.C., Int. J. Plasticity, 7, 803, 1991. With permission from Elsevier).

The accuracy and the numerical value of the elastic modulus are highly dependent upon the number of data points used in the least square analysis. A different number of data points leads to different values for the elastic modulus, and also leads to different initial zero offset strains. The zero offset strain is shown in (7.1) to affect the amount of proof strain. This effect is quite signiﬁcant, especially when the proof strain is as small as 5µ. In an effort to estimate the range of variation in the elastic modulus and the zero offset strain with respect to the number of data points used in the least square analysis, a strain domain, Dε , is deﬁned in the strain space and shown as AB in Figure 7.1(b). Data points lying between A and B are used in the least square analysis. All data points of this domain are within the elastic region. OP represents a probing path of proportional straining on which a

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

327

yield point Y is to be determined. Point O indicates the point from which the probe emanates, and it may differ from the strain-free origin in the case when subsequent yield surfaces are to be determined. Considering a pure torsion test, Wu and Yeh [4] found that ε R varies up to 5µ when Dε is < 0.01%, but the variation is still 2 to 3µ even with Dε >0.01%. This amount of variation is large indeed when the deﬁnition of yield is set at 5µ. Adding to the complication is the fact that the slope of elastic loading associated with probes of different paths may be slightly different from one another. This was experimentally veriﬁed by Ivey [6] and Wu and Yang [7]. Ivey reported that when a specimen of 2024-T4 aluminum was subjected to prestrain in tension followed by a pure torsion while keeping the tensile strain constant, the shear modulus varies by an amount depending upon the magnitude of the prestrain in tension. Wu and Yang found that, for a one-dimensional tension–compression test, the slope of the unloading curve at various strain was not quite the same levels for both 6061-T6 aluminum and 4142 steel. Thus, the elastic modulus and the zero offset strain ε R vary from one probe to the other, and their magnitudes should be determined for each path. However, this is usually not practical and not accounted for in the experiments. Therefore, this effect contributes to the data scatter of yield surfaces.

7.2.1.2

The effect of strain domain on the yield stress

As the elastic modulus and the zero offset strain are affected by Dε , the equivalent plastic strain is affected through an equation similar to (7.1). Consequently, the yield stress thus determined is also affected. The yield stress determined in the previously mentioned pure torsion test with varied Dε but a constant Rε of 0.01% shows severe ﬂuctuations when the strain domain Dε is very small, and it becomes steady when Dε is greater than approximately 0.01%.

7.2.1.3 The effect of probing path In order to minimize the effect of probes, consecutive probes are chosen not to be on the same side of the yield surface. Yet, the effect of probes is still signiﬁcant in that radial and nonradial probing paths do not lead to consistent yield points. This assertion is substantiated by the results of an experiment involving strain paths oa, obc, and ode illustrated by Figure 7.1(c). In the radial probe oa, the yield point was determined at “a” and any point beyond this point is in the postyielding state. Consequently, the point “p” of the line “bc” is considered to be in a yielded state. However, as judged by the probe of nonradial path obc, this particular point “p” was still in the elastic region. Point “c” was the yield point for this path. The yield point of path ode was determined to be at e. Figure 7.1(c) has thus demonstrated the probing path dependence of the yield point when it is determined by a small proof strain of 5µ.

© 2005 by Chapman & Hall/CRC Press

328

Continuum Mechanics and Plasticity

7.2.1.4 The effect of strain rate in probing It is known that some metallic materials exhibit signiﬁcant strain-rate effect even at room temperature, as mentioned in Section 5.2.4. The experimental constant strain-rate stress–strain curves show that stresses at different strain rates are signiﬁcantly unequal only in the postyielded range and thus a large offset strain deﬁnition of yield would lead to a yield stress which is quite strain-rate dependent. However, a rather weak rate sensitivity is evident when a small proof strain is used. It is thus reasonable to assume that for a proof strain as small as 5µ, the strain-rate effect in the probing is negligible. A similar conclusion was drawn by Ellis et al. [8] in connection with their testing of 316 stainless steel. For the range of probing rate (100 to 500 µε/min) used, the writers concluded that the probing rate had little effect on yield behavior and that the difference in size and position of the yield surfaces they determined was more related to the sequence in which the yield surfaces were determined rather than the probing rate.

7.2.2

A Summary of Experiments Related to the Determination of Yield Surfaces

Extensive literature is available on the issue of experimental determination of yield surfaces, with prestrains (i.e., specimen subjected to strain before a yield surface is determined) within the strain range (2% or less) of an electricalresistance strain gauge. The experimental works described here were carried out at room temperature. Most experiments were conducted using thinwalled tubes subjected to combined tension and torsion. This group includes Taylor and Quinney [9], Naghdi et al. [10], and Ivey [6] with prestrain in torsion; McComb [11] with prestrain in tension; Mair and Pugh [12] with prestrain in tension, partially unloaded and then strained in torsion; Bertsch and Findley [13] with zigzag paths in small steps; Phillips and Moon [14], Phillips and Lu [5], Shiratori et al. [15], and Ishikawa [16] with various prestrain histories; Wu and Yeh [4] with proportional paths of loading-unloading-reloading-cyclic steady state. Experiments were conducted by Lode [17] and Hu and Bratt [18] using thin-walled tubes subjected to tension and internal pressure. Plate specimens were used by Szczepinski [19], Szczepinski and Miastkowski [20], and Shiratori and Ikegami [21]. The experimental results generally conﬁrmed that the initial yield surface is closed to the Mises ellipse and the subsequent yield surfaces are obtained from the expansion in size, the motion, and distortion of the Mises ellipse. If the yielding is deﬁned using a small (5 to 10µ) proof strain, then the size of the ellipse does not change, that is, no cross effect has been observed. The discussion in this section is devoted to the effect of loading path on the yield surface, which includes the stress-controlled path and the strain-controlled path. The path may be linear or nonlinear, and a proportional strain path may not lead to a proportional stress path depending on material tested.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

329

(2)

(6)

(7) (3)

A

(5)

B

(4)

(1) O

D

C

FIGURE 7.2 Loading paths for combined axial–torsion.

7.2.2.1 Proportional path The proportional path includes monotonic axial loading, path (1) of Figure 7.2, monotonic torsion loading, path (2), and proportional combined tension and torsion, path (3). Most early works reported in the literature were conducted using load-control machines and were therefore controlling the stress path. Servo-controlled hydraulic test machines have been used in more recent works and stress- or strain-controlled tests are possible. Both cases (i.e., stressor strain-control) lead to the same result for monotonic axial loading and monotonic torsion in the small strain range. Phillips and Tang [22], Ishikawa [16], and most experiments reported in the literature used a prestress path. Wu and Yeh [4] used prestrain paths for monotonic axial and monotonic torsion prestrains, but a prestress path for a combined tension and torsion proportional loading. A conclusion arrived at from all available experimental data is that the yield surface undergoes kinematic hardening along the direction of loading and gets distorted with the “ﬂattened rear part” of the yield surface facing the origin of the stress space. The extent of kinematic hardening and the amount of isotropic hardening depend√upon the material tested and upon the deﬁnition yield. Thus, if plotted in the 3τ versus σ space, where τ is the shear stress and σ the axial stress, the initial yield surface for an initially isotropic material is a circle and the subsequent yield surfaces can be approximately described by ﬂattened ellipses. In a combined tension–torsion proportional loading, the initial yield surface, which is a circle, will gradually become distorted as the prestrain increases, with the ﬂattened ellipse facing the origin of the stress space. Note that this ﬂattened ellipse is a result of distortion and not a rotation of the yield surface. In fact, it is fair to say that no rotation of yield surface occurs during proportional loading. Subsequent yield surfaces with proportional prestrains are shown schematically in Figure 7.3. We note that some subsequent yield surfaces in the literature show a “rounded nose” in the direction of prestressing but a ﬂat rear on the side opposite to the prestress (see the solid curves), but some reported experimental yield surfaces do not

© 2005 by Chapman & Hall/CRC Press

330

Continuum Mechanics and Plasticity 3

O

FIGURE 7.3 Subsequent yield surfaces with proportional prestrain.

A

D

C

O

B

FIGURE 7.4 Loading point and yield point.

show these characteristics (see the dashed curves). The reason for differences is related to the point picked as the yield point when reloading takes place in the yield surface probing. Referring to Figure 7.4, the material is ﬁrst loaded from O to A, which moves the yield surface to its current state. Partial unloading from A to B would put the stress point at the center of the current yield surface. BCD represents the probing of the current yield surface and C is the yield point. If point A, which is known as the loading point is considered a point on the yield surface, then the yield surface will show a rounded nose. On the other hand, if C is considered a point on the yield surface, then the yield surface does not show a rounded nose. Some authors [14] distinguish between these two points and consider the ideas of loading surface and yield surface. But most experimental results found in the literature do not make this distinction. In the case of combined axial–torsion, only three papers have reported test results on proportional loading into the large strain range and they are discussed here. Helling et al. [23] conducted stress-controlled tests on several © 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

331

materials and obtained √ data showing the evolution of yield surface up to a shear prestrain of γ / 3 = 0.32 under torsion, path (2) of Figure 7.2. The paper did not specify whether they were free- or ﬁxed-end torsion tests. But since the authors did not report the axial stress during the torsion test, one can assume that the tests were conducted under the free-end torsion condition. The results are similar to those obtained in the small strain range, except that isotropic hardening is signiﬁcant for some materials. The paper did not discuss path (1) — monotonic axial preloading — but it did report a case of proportional loading, path (3), with a result similar to those observed in small strain. The ﬂattened ellipse was facing the origin of the stress space. However, this case was conducted with an effective prestrain of only 5%, which is small. Wu et al. [24] tested annealed 304 stainless steel and determined the initial and subsequent yield surfaces for two loading paths. Path (1) in axial loading had an axial prestrain of 20% and path (2) in free-end torsion had a shear prestrain of 20%. Experimental results showed that both the forward and rear parts deﬂated as the loading proceeded. These results contradict what is known at the small strain level, where the forward part inﬂates. In addition, for a prestrain of only 20%, the cross effect is very signiﬁcant for the material tested. This cross effect was not apparent in the work of Wu and Yeh [4] for the same material at small strain level. The experiments reported in Wu [25] provide another set of test data related to the evolution of yield surface with large prestrains. In the experimental determination of subsequent yield surfaces, a major difﬁculty is that strain gauges used to probe the previous yield surface are no longer functional when subsequent prestrain for the next yield surface exceeds 2%. Since the same specimen is used to determine several subsequent yield surfaces, the sum of all preloading (or prestrains) is the prestrain before next yield surface probing. The method used to overcome this difﬁculty was to unload the specimen after the specimen had been subjected to a predetermined amount of prestrain. The specimen was then removed from the test machine and new strain gauges were installed and cured. The specimen was then mounted again on the test machine and gradually loaded to merge with the stress–strain curve of prestraining, monitored by an axial–torsional extensometer designed and built by Wu and Xu [26]. At this point, a subsequent yield surface was probed using the newly installed strain gauges. The same method was used to determine other subsequent yield surfaces. Experiments were conducted for path (1) up to an axial prestrain of ε = 0.45 and for path (2) up to a shear prestrain of γ = 0.4. The test for path (2) was conducted under the free-end torsion condition. Note remarked that the test data for both paths (1) and (2) enable the determination of a complete set of parameters that can be used to calculate the combined axial–torsion response of the tube. Owing to prestrains into the ﬁnite deformation range, the expansion (or contraction) of yield surfaces is signiﬁcant for the materials tested by Helling et al. [23], Wu et al. [24], and Wu [25], even though yield was determined by a proof strain of 5µ. © 2005 by Chapman & Hall/CRC Press

332

Continuum Mechanics and Plasticity 3 Surface A

Surface B

Initial Yield Surface

O

FIGURE 7.5 Evolution of yield surface for tor–ten path (4).

7.2.2.2 Stress-controlled torsion–tension path Two stress-controlled torsion–tension paths (tor–ten for short) are meaningful. These paths are illustrated in Figure 7.2. Path (4) denotes a path with pretorsion from O to A, followed by an elastic unloading to an approximated center of the current yield surface at B. Axial loading is then applied, keeping the shear stress constant at the value of τB . Path (5) denotes a path with pretorsion from O to A, followed by an axial loading while keeping the shear stress constant at the value of τA . The tor–ten path (4) has been investigated by several investigators, including Phillips and Tang [22], Shiratori et al. [15], Ishikawa [16], and Helling et al. [23]. Figure 7.5 shows schematically the evolution of the yield surface for tor–ten path (4). Test results show that the yield surface (Surface A) at the end of the pretorsion stage serves as the basis for the subsequent yield surfaces (Surface B) generated by tension. The surface ﬂattens without rotation as the axial stress increases. All results have been obtained in the small strain range, including the tests of Helling et al. [23] for this case. No experimental data for the large strain range has been found in the literature for this test. Tor–ten path (5) has been investigated by Helling et al. [23]. The data have been obtained for tests up to a total prestrain (torsion and tension) of only 5%. Test results shows a rotation of yield surface as the axial stress increases. The yield surfaces of path (5) are shown schematically in Figure 7.6. Surface A denotes the yield surface at the end of the pretorsion stage and Surface B the yield surface after tensile stressing has been applied. 7.2.2.3 Stress-controlled tension–torsion path The stress-controlled tension–torsion paths are the counter part of the stresscontrolled tor–ten paths. Results should be similar in nature to those discussed

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

333 3 Surface A Surface B

O Initial Yield Surface

FIGURE 7.6 Evolution of yield surface for tor–ten path (5) (From Helling, D.E. et al., J. Eng. Mater. Technol., 108, 313, 1986. With permission from ASME).

in Section 7.2.2.2. There are two cases: path (6) denotes a path with pretension from O to C (see Figure 7.2), followed by an elastic unloading to an approximated center of the current yield surface at D. Torsion loading is then applied while keeping the axial stress constant at the value of σD . Path (7) denotes a path with pretension from O to C, followed by a torsion loading while keeping the axial stress constant at the value of σC . Path (6) has been investigated by several investigators, including Phillips and Tang [22], Shiratori et al. [15], and Ishikawa [16], and path (7) has been investigated by Helling et al. [23]. These investigations have all been conducted with prestrains in the small strain range. 7.2.2.4

Other paths

Experiments have been conducted following other stress-controlled paths and some with unloading and cyclic loading. However, the investigators were interested in other aspects of plastic behaviors and no information about the corresponding yield surfaces was reported. The investigations associated with the variation of plastic strain increment along a stress path will be discussed in the next section, related to the experimental investigation of the ﬂow rule. Strain-controlled loading paths have been used by several investigators to investigate the stresses arisen from the strain-path. The purpose of these experiments was to determine the relationship between stress components and the given plastic strain increment and was not related to the determination of yield surface. These experiments will be discussed in Section 7.5. 7.2.3

Yield Surface Versus Loading Surface

Based on experimental observations, Phillips and his coworkers proposed the idea of loading surface. A description of two-surface theory may be found in

© 2005 by Chapman & Hall/CRC Press

334

Continuum Mechanics and Plasticity 3

C

A b a

O II

I c

III

B d D

FIGURE 7.7 Motion of yield surface and the loading surface (From Phillips, A., Int. J. Plasticity, 2, 315, 1986. With permission from Elsevier).

Phillips [27]. The main concept that is different from the traditional concept of plasticity is to consider plastic ﬂow as rate dependent. Plastic strain takes time to develop and the existence of an equilibrium stress is postulated at which plastic strain is fully developed, see Wu [28], Phillips and Wu [29], Phillips [30], and Krempl [31]. A loading surface represents the largest state of stress achieved in the loading history, and it expands isotropically upon loading. Figure 7.7 shows the motion of the yield surface and the loading surface in the stress space. The yield surface tends to become tangential to the loading surface when it moves towards the loading surface. But, when the stressing point penetrates the loading surface, it will drag the loading surface with it and the loading surface expands. Referring to Figure 7.7, the initial yield surface which is also the initial loading surface is denoted by I. A stress path from O to A will cause the loading surface to expand to the surface labeled as II, and a stress path AD will cause the loading surface to expand further to Surface III. On the other hand, stress path AC does not cause the loading surface to expand because path AC does not penetrate the corresponding loading surface, Surface II. Surfaces labeled as a, b, c, and d are yield surfaces. Since plastic strain takes time to develop, the experimentally determined yield surface after path OA is Surface a only after the stressing point has stayed at A for a sufﬁcient length of time. If the prestress point does not stay at A for a sufﬁcient length of time before the yield surface is probed, then the obtained yield surface will

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

335 T T1

Troom

3

FIGURE 7.8 Yield Surface in the stress–temperature space (From Phillips, A., Int. J. Plasticity, 2, 315, 1986. With permission from Elsevier).

be a distance away from the loading surface and does not touch the loading surface. 7.2.4

Yield Surface at Elevated Temperature

Phillips and his coworkers [32–35] conducted a series of experiments and determined yield surfaces at elevated temperatures which were lower than 0.3Tm , where Tm is the absolute melting temperature of the material. Thinwalled tubes of 1100-0 aluminum were tested. The yield surface in the stress–temperature space is shown schematically in Figure 7.8, where the surface is depicted between two constant temperatures T1 and Troom with T1 > Troom . An isothermal yield surface may be obtained by passing a plane normal to the temperature axis. The yield surface (the isotherm) shrinks as the temperature increases. The yield surface is actually a conoid with a ridge at the top. The length of the ridge depends on the prestrain history, measured by equivalent plastic strain. The initial yield surface is a cone with an elliptical base. The length of the ridge is zero because the equivalent plastic strain is zero. As the equivalent plastic strain increases with the prestraining history, the length of the ridge also increases with a narrower width for the corresponding isothermal yield surfaces. A ridge is formed when the width of the isothermal yield surface at the top is zero. The ridge is perpendicular to the direction of preloading. For each value of equivalent plastic strain, there corresponds a temperature Tmax which deﬁnes the height of the conoid with a ridge at the top. The temperature Tmax decreases with the increasing equivalent plastic strain. Finally, we mention that the distortion and motion of the yield surface can occur either by an increment of loading history or by a temperature increment or by a combination of the two. Figure 7.9 shows a case of initial and subsequent isothermal yield surfaces determined by Phillips and Tang [22] at 21, 66, 108, and 152◦ C (70, 151, 227, and 305◦ F) due to prestress in tension.

© 2005 by Chapman & Hall/CRC Press

336

Continuum Mechanics and Plasticity

2.0

6 A⬘ 10 22

1.0

227

30

Shear Stress (KSI)

26

0

3 28 227°F

14 18

°F

5°F

27 23 19 75 8 17 21 25 29

305°F

–1.0

Specimen S–5

70°F 151 °F

13 16

9 12

24

20

151°F 15

70°F 7 A⬘

2×

4

A

First Sub Yield Surface Prestressing at A 2 = 5507 lb/in T = 70°F p = 45 µ⬙/u

11

Initial Yield Surface –2.0 0

1.0

2.0

3.0

4.0

5.0

6.0

Tensile Stress (KSI)

FIGURE 7.9 A case of initial and subsequent isothermal yield surfaces (From Phillips, A. and Tang, J.L., Int. J. Solids Struct., 8, 463, 1972. With permission from Elsevier).

7.3

The Direction of the Plastic Strain Increment

It was mentioned in Section 6.3 that an important assumption concerning p the plastic strain increment dεij is that the principal axes of plastic strain increment and deviatoric stress are coincident, which is known as the norp mality rule and which says that dεij is normal to the yield surface. It was also mentioned that this assumption has been experimentally veriﬁed. But, it is to be emphasized here that those veriﬁcations were valid for initial yield surface p only. The following question remains: Is dεij normal to the subsequent yield surface? A direct answer can be found from the works of Phillips and Moon [14] and Ohashi et al. [36] who showed that the plastic strain increment is indeed normal to the subsequent yield surfaces. Figure 4 of Phillips and Moon [14] is reproduced as Figure 7.10. In the ﬁgure, the initial yield surface is labeled as 0 and the ﬁrst prestressing path is OA. The yield surface corresponding to A is labeled as I. In this discussion, we do not emphasize the difference between a loading surface and a yield surface as the writers did. The next stage of stressing went from B to C in tension. Path BC is nearly tangential to the ﬁrst subsequent yield Surface I. The second subsequent yield surface labeled as II was then determined. This surface

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

337

4

3

A I

2

II B

C

× 10–3 psi

1 III 0 0

D

3

4

5

6 × 10–3 psi

7

–1 IV –2 E –3

–4

Specimen M-3

FIGURE 7.10 Plastic strain increment vector (From Phillips, A. and Moon, H., Acta Mech., 27, 91, 1977. With permission from Springer).

shows further distortion from the previous surface and it translated not only in the direction of prestressing but also by a small amount in the direction perpendicular to the prestressing direction. Owing to the distortion, it is difﬁcult to judge whether rotation had taken place in yield Surface II. The directions p of dεij along path BC are also shown in the ﬁgure. These directions rotated from the direction normal to the yield surface from which the prestressing was initiated to the direction normal to the ﬁnal yield surface. We note that this stress path is similar to tor–ten path (5) discussed in Section 7.2.2.2. The second stage of both paths is tangential to the yield surface. The only difference is that the path of Phillips and Moon started from the opposite side of the ﬁrst subsequent yield surface, while path (5) starts from the prestress point A. Another stress, similar in nature, is shown in Figure 7.10. Starting from the yield surface labeled as III, stress path DE was applied. This stress path was again nearly tangential to the yield surface. At the end of the stressing, a yield surface was determined and labeled as IV. A distortion of yield surface had taken place and the surface had moved not only in the direction of prestressing but also in the lateral direction. Owing to the distortion, it is difﬁcult to judge whether the yield surface had rotated. Small vectors in the p ﬁgure show the variations in the direction of dεij .

© 2005 by Chapman & Hall/CRC Press

338

Continuum Mechanics and Plasticity 3 – 139°

131°

120° 107°

150°

100° 90°

1.0

B 164°

60° A

0.5

30° I = 4 3 2 1 0.5 0.2 0.1 0.05 180°

0.02% 0°

–10

–0.5

0

0.5

1.0

–

z/

FIGURE 7.11 Plastic strain increment vector (From Ohasi, Y. et al., J. Mech. Phys. Solids, 23, 277, 1975. With permission from Elsevier).

Ohashi et al. [36] prestressed a tubular specimen in tension (ﬁrst stress path) to a tensile stress of σz /σ¯ = 1.0, where σ¯ = 235 MPa. The corresponding prestrain at this point was 2%. A second stress path was then applied in combined axial–torsion, emanating from the prestress point making an angle θ with the ﬁrst stress path. Figure 3 of Ohashi et al. [36] is shown as Figure 7.11, in which θ = 0, 30, 60, 90, 100, 107, 120, 131, 139, 150, 164, and 180◦ . The strain data along each stress were recorded and the equi-strain curves √ path p 2 p 2 1/2 based on Iε = {(ε ) + (γ / 3) } and corresponding to Iε = 0.02%, 0.05%, 0.1%, 0.2%, 0.5%, and 1%, 2%, 3%, and 4% are found and shown in the ﬁgure. These curves are similar to subsequent yield surfaces determined by the use of different amounts of proof strains, and these are yield surfaces corresponding to the prestress point at σz /σ¯ = 1.0. The short segments on the second stress path√for each θ show the directions of the plastic strain increment vector (γ p / 3, εp ). Ohashi et al. [36] found that the plastic strain increment vector is almost normal to the equi-strain curves, except for the range of Iε ≤ 0.05% and 139◦ < θ < 164◦ . Other investigations of the plastic strain increment did not report the yield surfaces along the stress paths and therefore the information provided is not complete enough to directly beneﬁt the constitutive modeling. Nevertheless, these works are useful in that they can provide qualitative results for certain observed behaviors of materials. Phillips and Kaechele [37] conducted stresscontrolled tests on thin-walled tubes of aluminum 2S-O following tor–ten path (5) and ten–tor path (7). The tests were conducted in a strain range √ up to 1.5%. The stress paths are shown schematically in Figure 7.12 in the ( 3τ , σ ) space. The short segments on the √ stress paths show the directions of the plastic strain increment vector (γ p / 3, εp ). For tor–ten path (5), the plastic strain increment was along the shear direction before a sudden change of direction

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

339 3

O

FIGURE 7.12 Plastic strain increment vector (From Phillips, A. and Kaechele, L., J. Appl. Mech., 23, 43, 1956).

3 D

C F

E

O

B

A

FIGURE 7.13 Stress paths of Khan and Wang (From Khan, A.S. and Wang, X., J. Mech. Phys. Solids, 36, 519, 1988. With permission).

took place in the stress path. The direction of the plastic strain increment gradually changes afterward. In the case of ten–tor path (7), the plastic strain increment was initially along the tension direction and the direction gradually changes after the change in direction of the stress path. Khan and Wang [38] conducted combined axial–torsion tests on OHFC copper, following two stress paths shown in Figure 7.13. In path OABC, the specimen was ﬁrst stressed in tension to A into the plastic region. Partial unloading and reverse loading then took place from A to B while keeping the shear stress zero. Finally, torsion was increased from B to C while keeping the axial stress constant. In path ODEF, the specimen was subjected to shear stress from O to D, unloading from D to E, and then loading from E to F. The two paths are similar in nature. The corresponding strain paths are shown schematically in Figure 7.14. From the ﬁgure we see that during segment BC of path OABC, the increment of axial strain ε changes from negative to positive as the shear stress increases while keeping the axial stress σ constant. Similarly, during segment EF of path ODEF, the increment of shear strain γ changes from negative to positive as the axial stress increases while keeping

© 2005 by Chapman & Hall/CRC Press

340

Continuum Mechanics and Plasticity 3

E

F C

O

B

FIGURE 7.14 The corresponding strain paths of Khan and Wang (From Khan, A.S. and Wang, X., J. Mech. Phys. Solids, 36, 519, 1988. With permission).

the shear stress τ constant. The curves have been exaggerated to show the sign change in dε and dγ .

7.4

Multisurface Models of Flow Plasticity

It was mentioned in Section 7.2.3 that Phillips [27] proposed a multisurface model in which the yield surfaces are bounded by the loading surface. However, in most of the investigations by Phillips, emphasis was placed on how to describe the change of the yield surface and the direction of the plastic strain increment. Little was done to propose and verify the ﬂow rule in terms of plastic modulus, particularly for complex loading paths including unloading and reloading. With a correctly determined plastic modulus, the ﬂow rule should describe the nonlinear stress–strain curves. Multisurface models that attempt to accomplish just that are discussed in this section. These models emphasize the description of cyclic loading behavior. 7.4.1

The Mroz Kinematic-Hardening Model

The work of Mroz [39] has a large following, particularly in computational mechanics. Mroz approximated the one-dimensional stress–strain curve OABCDE by n linear segments of constant tangent moduli E1 , E2 , . . . , En , as in Figure 7.15. The tangent modulus decreases as the strain increases. This is the idea of a “ﬁeld of work-hardening moduli.” If the stress–strain curve of Figure 7.15 is projected onto the stress space, then we have a one-dimensional stress space in the σ -axis. In the multidimensional stress space, this ﬁeld is deﬁned by a conﬁguration of surfaces of constant work-hardening modulus. Each nodal stress (stress at A, B, C, etc.) is represented by a surface

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

341

E

E9 E8

E6

E7

C5

C4

B3

C

B

D

A

O B1 B2

C3 E5

C2

C1

E1

E2

E3

E4

FIGURE 7.15 Mroz’s Field of work-hardening moduli concept.

geometrically similar to the initial yield surface but of different size. These surfaces are expressed by (m) 2 fm σij − αij = Ym

(7.2)

where m = 0, 1, 2, …. Using the Mises yield criterion, the surfaces are concentric circles in the two-dimensional stress space, as shown in Figure 7.16(a). Thus, surface fA is the initial yield surface passing through point A of Figure 7.15 and fB is the surface passing through point B, etc. In Mroz’s hardening rule, the surfaces cannot intersect but consecutively contact at similar points and push each other. Similar points are stress points on different surfaces with the same outward normal. During loading sequence OABCDE, surface fA translates so as to touch surface fB at the point of loading; next, surfaces fA and fB move together until they contact surface fC , and so on. The surfaces at stress state C are shown in Figure 7.16(b). Since all surfaces can contact only at the similar points, the active surface translates in the direction parallel to the vector connecting the current stress point σm to the corresponding similar point σm+1 of the next surface. This hardening rule is expressed by dαm = dµ (σm+1 − σm )

(7.3)

where dµ is a scalar to be determined by the consistency condition; dαm describes the translation of the active surface fm . Figure 7.17 is a sketch of Mroz’s hardening rule.

© 2005 by Chapman & Hall/CRC Press

342

Continuum Mechanics and Plasticity 2

(a)

E D C B A

fC fD

fA

(b)

E

1

fB

O

fE

(c) C

D C

C5

fE fD

C4

fC fB

fA fB C1 C2 C3

fC

fA fD

fE C3

FIGURE 7.16 (a) A family of concentric circles, (b) surfaces at stress state C of Figure 7.15, (c) surfaces at stress state C3 of Figure 7.15.

The discussion of the one-dimensional loading shown in Figure 7.15 is continued here. After reaching stress state C shown in Figure 7.16(b), if unloading takes place, then the stress point will move from C to C1 elastically. Reverse plastic ﬂow occurs at C1 and surface fA translates downwards until it contacts surface fB at C2 . We see from the ﬁgure that the stress difference between C1 and C2 is twice that between A and B. Further unloading from C2 to C3 will induce additional plastic deformation and the stress point carries surfaces fA and fB with it until it contacts surface fC at C3 . This state of stress is shown in Figure 7.16(c). We mention again that the stress difference between C2 and C3 is twice that between B and C. The reloading from C3 to C4 is again elastic, but plastic deformation occurs from C4 to C5 . The stress point carries surface fA with it until it contacts surface fB . Further loading from C5 to C translates both

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

343 m + 1

m d

m

m + 1 fm

fm + 1

Stress Space FIGURE 7.17 Mroz’s hardening rule.

C n P

R

n

Q

S n T

fA fB fC FIGURE 7.18 A case of nonproportional loading (Mroz’s model).

fA and fB and returns the stress state back to C, as shown in Figure 7.16(b). We have thus completed one cycle of loading–unloading–reloading. Additional loading cycles follow the same path C–C1 –C2 –C3 –C4 –C5 –C and this is the steady loop and no cyclic hardening is possible by use of Mroz’s model. We also show in Figure 7.15 a steady loop with unloading starting at B and a loop with unloading starting at E. Looking at a loop of cyclic loading, we ﬁnd that the difference in stress for each piecewise-linear step during unloading or reloading is twice that of the corresponding step during loading. The difference in the strain for each step also has the same characteristic. We may conclude that the slopes of E1 E2 and E6 E7 are the same as that of AB, and the slopes of E2 E3 and E7 E8 are the same as that of BC, etc. In fact, the loading, unloading, and reloading curves are similar and they satisfy Masing’s formula [40]. A case of nonproportional loading is now considered. Upon loading to C as in Figure 7.16(b), the specimen is partially unloaded to a point P, Figure 7.18.

© 2005 by Chapman & Hall/CRC Press

344

Continuum Mechanics and Plasticity

The stress point then moves along PQ, and when it reaches point R, it will move along the direction of RS. The normal to surface fB at S is the same as the normal to surface fA at point R. S is the point at which fA will be tangential to and not intersecting fB . In the next step the stress point will move from S to T. Again, the normal to fC at T is parallel to the normal previously mentioned at R and S. The work-hardening modulus on this loading path decreases and becomes equal to that at C when the stress path intersects fC at T. Mroz [39] used this example to illustrate a case of nonproportional loading. We remark that the stress path after the partial unloading is PRST and not PRQ. In a stresscontrolled tor–ten test, with stress point moving along PQ as in paths (4) and (5) of Figure 7.2, the contact between fA and fB takes place at a location other than S. 7.4.2

The Two-Surface Model of Dafalias and Popov

Dafalias and Popov [41,42] proposed a two-surface model and deﬁned a continuous variation of the plastic modulus dσ/dε p = Ep between these two surfaces. This is in contrast to Mroz’s model presented in Section 7.4.1, which proposes a piecewise constant plastic moduli ﬁeld and a number n of associated surfaces. In the two-surface model a bounding surface is proposed in the stress space in addition to the yield surface (sometimes also called the loading surface). The loading surface is used interchangeably with the yield surface in this discussion and does not have the same meaning as that deﬁned by Phillips, mentioned in Section 7.2.3. The bounding surface always encloses the yield surface and is a generalization of the bounds observed in the experimental results for uniaxial random cyclic loading on a grade 60 steel specimen. The details of the experimental random cyclic loading curve were presented in [41]. Figure 7.19 shows a simpliﬁed schematic cyclic curve with some parameters of the model indicated. Lines XX and YY are the bounds for the material tested. They can be curves for other materials. Curve 0–1–2 is a loading stress–plastic strain curve and it merges with the bounding line XX when the loading continues. If unloading occurs at point 2, then the unloading curve would follow 2–3–4 and merge with the bound line YY . On the other hand, if reloading starts at A, then AB is elastic and plastic deformation begins to occur at B. Experimental results indicated that the curve after B is steeper than curve Section 3–A, that is, the plastic moduli are not of the same magnitude between the two curve sections. Dafalias and Popov [41,42] suggested that Ep be a function of two parameters, the distance δ of the stress state under con¯ and the value sideration, such as point A, from the corresponding bound A, of δ at the initiation of yielding for each loading process, denoted by δin . The δin changes at each reversal and is associated with the most recent event of unloading–reloading. In fact, this is an assumption of fading memory, where the material remembers only the most recent loading history. Thus, we write Ep = Ep (δ, δin )

© 2005 by Chapman & Hall/CRC Press

(7.4)

Advances in Plasticity

345 2

B

b

X⬘

b

X

B

1

3

O

p

in A

a a Y⬘

Y

A

4

FIGURE 7.19 Bounds and parameters of two-surface model.

with the property that Ep → ∞

when δ → δin

(7.5)

for a smooth transition from the elastic into elasto-plastic range and E¯ p = Ep (0, δin )

when δ → 0

(7.6)

where E¯ p is the slope of the bound line and Ep monotonically increases as δ decreases. Dafalias and Popov [42] recommended the following expression for Ep : δ Ep = E¯ p + h (7.7) δin − δ where h is a function of δin and a nonlinear form for h has been chosen to model the complex random cyclic loading curve presented in Dafalias and Popov [41]. ¯ and B¯ are projected onto the Referring to Figure 7.19 again, points A, B, A, ¯ a and stress axis and the corresponding points are denoted by a, b, a¯ , and b. b are points on the yield surface, whereas a¯ and b¯ are points on the bounding surface. The rates of change of centers of yield and bounding surfaces are related to the plastic strain rate by α˙ = Eα ε˙ p

© 2005 by Chapman & Hall/CRC Press

(7.8)

346

Continuum Mechanics and Plasticity

and β˙ = Eβ ε˙ p = α˙ − (Eα − Eβ )˙ε p

(7.9)

respectively. When there is no isotropic hardening of the yield surface, Eα = Ep ; and when there is no isotropic hardening of the bounding surface, Eβ = Ep . In this case, the two bounds are parallel straight lines in the one-dimensional case. In the multiaxial stress space, the yield surface f and the bounding surface f¯ are f (σij − αij , qn ) = 0

and

f¯(σ¯ ij − βij , qn ) = 0

(7.10)

where αij and βij denote the centers of f and f¯, respectively, and qn are internal variables (which will be further discussed in Chapter 8). The two surfaces may deform and translate in stress space in a coupled way. The evolution of qn is given by q˙ n = q˙ n (σij , σ˙ ij , qm , ξm )H(L)

when f = 0

q˙ n = 0

when f < 0

(7.11)

where H(L) is the Heaviside step function and L is the loading function, which under the isothermal condition is L = σ˙ = σ˙ ij nij

(7.12)

in which n is the unit normal to the yield surface. Internal variables qn represent the dependence of the yield surface on the history of deformation. One of the qn may describe isotropic hardening. ξm in (7.11) are internal variables associated with abrupt changes of the loading processes. In the present case, they are the δin ’s. These parameters remain constant during the loading process. The continuously changing δ and the initial value δin deﬁne the generalized plastic modulus K with the properties K = K(δ, δin ),

K¯ = K(0, δin ),

K(δin , δin ) = ∞

(7.13)

where K¯ is the generalized plastic modulus on the bounding surface and is an increasing function of δ for a given δin . The distance δ is from point a on the yield surface f = 0 to a similar point a¯ on the bounding surface f¯ = 0 (see Figure 7.20). At similar points, the normals to the respective surfaces are equal. Let the stress at point a be σij and the stress at point a¯ be σ¯ ij , then δ is deﬁned by δ = [(σ¯ ij − σij )(σ¯ ij − σij )]1/2

© 2005 by Chapman & Hall/CRC Press

(7.14)

Advances in Plasticity

347 22

a

ij ij a

Yi e l d

ac

ij

e

ij

nij

Su

rf

11

O u rf gS B o undi n

ac e

FIGURE 7.20 Two-surface model in two-dimensional stress space (From Dafalias, Y.F. and Popov, E.P., J. Appl. Mech., 98, 645, 1976. With permission from ASME).

For simplicity, we assume that the bounding surface is an isotropic expansion of f = 0, but both surfaces are allowed to move. The centers for the two surfaces are αij and βij , respectively, as shown in Figure 7.20. Since the two surfaces are similar, the radii connecting the two centers and the corresponding stress points are parallel. Thus, it is written as σ¯ ij − βij = m(σij − αij )

(7.15)

where m is a proportional factor which can be a function of qn . This relation may be further written as σ¯ ij − σij = m(σij − αij ) + βij − σij

(7.16)

and be substituted into (7.14) to obtain an expression for δ. Several rules of evolution of αij and βij have been used in the literature in conjunction with the two-surface model. The following discussion follows p Dafalias and Popov [42]. Assuming linear dependence of ε˙ ij on the stress rate, the ﬂow rule, assuming normality, is p

ε˙ ij =

1 Lnij K

(7.17)

where is the Macauley bracket deﬁning the operation L = LH(L). From (7.17), we found p p 1/2 L = σ˙ = K ε˙ ij ε˙ ij

© 2005 by Chapman & Hall/CRC Press

(7.18)

348

Continuum Mechanics and Plasticity

Working with the magnitudes and projection of the stress rate onto the normal direction, this relation is a generalized relation of σ˙ = Ep ε˙ p in the onedimensional case, that is, Ep has been generalized into K. We now use the same procedure to generalize (7.8) by writing p p 1/2 Kα α˙ = α˙ ij nij = K α ε˙ ij ε˙ ij L = K

(7.19)

Denoting the unit vector along α˙ ij by νij , which is, in general, not in the same direction as nij , we may write α˙ ij = α˙ ν νij

(7.20)

where α˙ ν is the magnitude. Substituting (7.20) into (7.19), we have α˙ = α˙ ij nij = α˙ ν νij nij

(7.21)

α˙ 1 Kα νij = Lνij νrs nrs νrs nrs K

(7.22)

Therefore, α˙ ij =

The modulus K α /K can be determined by substituting (7.22) into the consistency condition. Referring to the yield surface given in (7.10), the consistency condition is ∂f ∂f ∂f f˙ = q˙ n = 0 σ˙ ij + α˙ ij + ∂σij ∂αij ∂qn

(7.23)

Denoting the magnitude of ∂f /∂σij by g=

∂f ∂f ∂σij ∂σij

1/2 (7.24)

we write ∂f = gnij ∂σij

(7.25)

In addition, we assume that q˙ n is linear in σ˙ ij , that is, q˙ n = rn L

(7.26)

where rn is a scalar. Using (7.24) to (7.26), (7.23) reduces to Kα 1 ∂f rn =1+ K g ∂qn

© 2005 by Chapman & Hall/CRC Press

(7.27)

Advances in Plasticity

349

We then substitute (7.27) into (7.22) to obtain α˙ ij . This relation applies to any kinematic-hardening rule for which νij is speciﬁed. A special case is obtained when ∂f /∂qn = 0. In this case, K α = K, which corresponds to Eα = Ep in the one-dimensional case. The same procedure may be used again to generalize (7.9). By differentiating (7.10), the consistency condition for the bounding surface is ∂ f¯ ˙ ∂ f¯ ∂f f˙¯ = σ¯ ij + β˙ij + q˙ n = 0 ∂ σ¯ ij ∂βij ∂qn

(7.28)

Writing

∂ f¯ ∂ f¯ ∂ σ¯ ij ∂ σ¯ ij

1/2

∂ f¯ = g¯ nij ∂ σ¯ ij

(7.29)

p p 1/2 K¯ L¯ = σ˙¯ = σ˙¯ ij nij = K¯ ε˙ ij ε˙ ij = L K

(7.30)

g¯ =

,

and

and using them in (7.28), the consistency condition is nij β˙ij = L¯ +

1 ∂ f¯ rn L g¯ ∂qn

(7.31)

We now generalize (7.9) to obtain p p 1/2 Kβ β˙ = β˙ij nij = K β ε˙ ij ε˙ ij = L K

(7.32)

and denote the unit vector along β˙ij by ξij , then β˙ij = β˙ ξ ξij

(7.33)

where β˙ ξ is the magnitude. But, β˙ is the projection of β˙ij along nij , and, therefore, we have β˙ = β˙ij nij = β˙ ξ ξij nij

and

β˙ ξ =

β˙ ξij nij

(7.34)

Hence, β˙ij =

© 2005 by Chapman & Hall/CRC Press

β˙ 1 Kβ ξij = Lξij ξrs nrs ξrs nrs K

(7.35)

350

Continuum Mechanics and Plasticity

For simplicity, consider a case νij = ξij = µij . This assumption is similar to Mroz’s hardening rule, where µij is a unit vector going from point a to point a¯ (see Figure 7.20). For this case, (7.22) reduces to α˙ ij =

1 Kα Lµij µrs nrs K

(7.36)

β˙ij =

1 Kβ Lµij µrs nrs K

(7.37)

and (7.35) reduces to

Analogous to the second expression of (7.9), we write β˙ij = α˙ ij − Mµij

(7.38)

From (7.36) to (7.38), the following is obtained M=

1 Kα − Kβ L µrs nrs K

(7.39)

Substituting (7.30), (7.38), and (7.39) into (7.31) obtains Kβ K¯ 1 ∂ f¯ = + rn K K g¯ ∂qn

(7.40)

Using (7.27) and (7.40), (7.39) may be further written as 1 M= µrs nrs

K¯ 1− K

+

1 ∂ f¯ 1 ∂f rn − rn g¯ ∂qn g ∂qn

L

(7.41)

In the case that both f and f¯ are not functions of qn , (7.41) becomes 1 M= µrs nrs

K¯ 1− K

L

(7.42)

¯ In the limit, when the yield surface contacts the and (7.40) yields K β = K. ¯ the two surfaces will then move together bounding surface, δ = 0, and K = K, upon further loading. From (7.36) and (7.37), we have β˙ij = α˙ ij

© 2005 by Chapman & Hall/CRC Press

(7.43)

Advances in Plasticity

7.5

351

The Plastic Strain Trajectory Approach

The strain (total strain, not plastic strain) trajectory approach was initiated by Ilyushin [43,44], who represented the stress and deviatoric strain tensors in a ﬁve-dimensional vector space. He then investigated the characteristics of the stress response to a predetermined strain trajectory. Further investigations using this approach are reported by Lensky [45] and Ohashi and his coworkers [3,36,46,47]. A theory by Pipkin and Rivlin [48] is similar to Ilyushin’s theory but using strain tensors, and Zhou et al. [49] consider the plastic strain trajectory. In an independent effort, Valanis [1,2] developed an endochronic theory of plasticity using irreversible thermodynamics of internal variables. The resulting constitutive equation, if expressed in an integral form, resembles that presented by Ilyushin [50]. In this constitutive equation, stress is a functional of the plastic strain history. The differences between the two developments will be addressed in Section 7.5.2. Wu and his coworkers [51–55] have contributed to the experimental veriﬁcations and applications of the endochronic theory. The endochronic theory of plasticity will be further discussed in Chapters 8 and 9. 7.5.1

The Theory of Ilyushin

Ilyushin worked with the deviator of the strain tensor (not plastic strain). When the strain is large, the plastic strain may be approximated by the total strain. The theory is, however, not suitable for describing the elastic–plastic transition behavior. The deviatoric strain eij has only ﬁve independent components. Thus, eij may be represented by a vector in a ﬁve-dimensional space as e=

5

ε i ui

(7.44)

i=1

in which ui are unit vectors along axes of the ﬁve-dimensional space. The magnitude of this vector must be equal to the magnitude of tensor eij , so that

eij eij ≡

i,j=1,2,3

If we deﬁne ε3 =

√ 2e12 ,

ε4 =

5

(εi )2

(7.45)

i=1

√ 2e23 ,

ε5 =

√ 2e31

(7.46)

then (7.45) and (7.46) are reduced to (e11 )2 + (e22 )2 + (e33 )2 = (ε1 )2 + (ε2 )2

© 2005 by Chapman & Hall/CRC Press

(7.47)

352

Continuum Mechanics and Plasticity 2⬘

6

2

3⬘

6 +

6

– 6

1⬘ 2 – 3

1

FIGURE 7.21 Coordinate transformation in the deviatoric strain plane.

The relationships between components of (ε1 , ε2 ) and (e11 , e22 ) are found from the coordinate transformation given in Figure 7.21. Note that e33 = −(e11 + e22 ). In the ﬁgure, axes 1 , 2 , and 3 denote the coordinate axes for e11 , e22 , and e33 , respectively, in the π -plane; whereas 1 and 2 denote the axes of ε1 and ε2 . The 1-axis is making angle β with the 1 -axis. Projecting ε1 and ε2 onto the 1 and 2 directions, respectively gives

e22

e11 = m(ε1 cos β + ε2 sin β)

π π = m −ε1 sin β + + ε2 cos β + 6 6

(7.48a) (7.48b)

where the factor m is introduced √so that (7.47) is satisﬁed. Substituting (7.48) into (7.47), we obtain m = 2/3. Using this value of m, we found from (7.48) that 3 = ε1 cos β + ε2 sin β e11 2

3 π π (7.49) e22 = −ε1 sin β + + ε2 cos β + 2 6 6

3 π π e33 = ε1 sin β − − ε2 cos β − 2 6 6 The third equation of (7.49) was found from e33 = −(e11 + e22 ). The ﬁrst two equations of (7.49) may then be solved to obtain

√

π − e22 sin β ε1 = 2 e11 cos β + 6 (7.50)

√

π ε2 = 2 e11 sin β + + e22 cos β 6

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

353

Finally, if the angle is set to β = 0, then we have ε1 =

√ 1 ε2 = 2 e22 + e11 , 2 √ √ ε4 = 2e23 , ε5 = 2e31

3 e11 , 2

√ ε3 = 2e12 ,

(7.51)

These are the ﬁve components in the plastic strain space.

+σ +σ = 0 may be represented Similarly, the deviatoric stress σij with σ11 22 33 in a ﬁve-dimensional stress space by the following components: σ1 =

√ 1

σ2 = 2 σ22 + σ11 , 2 √

√

σ4 = 2σ23 , σ5 = 2σ31

3

σ , 2 11

√

σ3 = 2σ12 ,

(7.52)

The next step is to establish a relationship between the stress and the strain increment, and this relationship is expressed in terms of the arc length s measured along the strain path. In the case of combined axial–torsion, the stress is (σ1 , σ3 ) and the strain increment is (dε1 , dε3 ). A plane strain trajectory is shown in Figure 7.22, and the arc length is ds =

(ε1 )2 + (ε3 )2

(7.53)

If the current strain state is represented by point A, unit vector p1 is tangential to the trajectory at A, and unit vector p3 is the principal normal. A similar ﬁgure is presented in [49] but in the plastic strain space. According to the Frenet formulas for curves in space, we have the following relations: dp3 = −κp1 ds

dp1 = κp3 , ds 3

p3

(7.54)

e3 A

p1 e1

Str ain

tr

e aj

ry cto

O

1

FIGURE 7.22 A plane strain trajectory and stress (From Zhou, Z.-D. et al., Int. J. Plasticity, 19, 1377, 2003. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

354

Continuum Mechanics and Plasticity

where κ is the curvature. Writing the stress vector as σ = Pp1 + Np3

(7.55)

Lensky [45] and Ohashi and his coworkers [3,36,46,47] conducted combined axial–torsion experiments to determine the variations of P, N, the magnitude of σ, denoted by σ , and the angle of delay θ between vectors σ and dε as functions of s. The angle of delay is found from cos θ =

σ · dε σ ds

(7.56)

These authors believe that these relationships are the constitutive equations of the material under investigation. Trajectories investigated include proportional strain trajectories, strain trajectories with two straight branches, orthogonal bilinear trajectories with a rounded corner, and more general curvilinear strain trajectories. The results show that the arc length s and the curvature κ are two important parameters deﬁning the constitutive behavior of the material. Ilyushin proposed a postulate of isotropy, see [45], which states that, for a strain trajectory starting from the origin of the strain space, the stress response is deﬁned by the intrinsic geometry of the strain trajectory and is invariant with respect to transformation of strain trajectory by means of rotation or reﬂection. Ilyushin further proposed the principle of delay, which states that the stress response to a strain trajectory is not deﬁned by the whole strain trajectory, but by the recent past of the trajectory with length λ known as the trace of delay. This is in fact a statement of fading memory. In the case of a curved trajectory followed by a straight trajectory, at a distance λ after the beginning of the straight trajectory, the stress vector becomes tangent to the trajectory. This is a very intuitive statement, because experimental results show that the stress path and the strain path do not coincide even for a proportional straining. Ilyushin [50] further proposed the following integral constitutive equation σ(s) =

0

s

K[s, s ; κi (s), κi (s )]dε(s ),

i = 1, 2, 3, 4

(7.57)

where s is the running parameter of integration; the kernel function multiplied by dε(s ) represents the contribution of dε(s ) to the stress vector at s ; and κi represents the geometry of the strain trajectory. A recent derivation of (7.57) by Zhou et al. [49] in the plastic strain space is now discussed with permission from Elsevier. p p Referring to Figure 7.22, in which the axes should be renamed ε1 and ε3 , the plastic strain increment is p

p

dεp = dε1 e1 + dε3 e3 = dsp1

© 2005 by Chapman & Hall/CRC Press

(7.58)

Advances in Plasticity

355

and the stress is σ = σ1 e1 + σ3 e3 = σ (cos θ p1 + sin θp3 )

(7.59)

where ei are base vectors of the Cartesian coordinate system; and θ is the angle of delay between vectors σ and dεp . We now deﬁne the length of the plastic strain path by ds =

p 2 p 2 ε1 + ε3

(7.60)

Differentiating (7.59) with respect to s and using (7.54), we obtain σ˙ = g1 p1 + g3 p3

(7.61)

where g1 = σ˙ cos θ − σ (κ + θ˙ ) sin θ ,

˙ cos θ g3 = σ˙ sin θ + σ (κ + θ)

(7.62)

We now make use of the transformation equations p1 = cos ηe1 + sin ηe3 ,

p3 = − sin ηe1 + cos ηe3

(7.63)

and the relations p

cos η =

p

dε1 , ds

sin η =

dε3 ds

(7.64)

and substituting (7.63) and (7.64) into (7.61) to obtain

p

p

dε dε σ˙ = σ˙ 1 e1 + σ˙ 3 e3 = g1 1 − g3 3 ds ds

p

p

dε dε e1 + g1 3 + g3 1 ds ds

e3

(7.65)

We have thus found from (7.65) that g dσ1 = 1 dσ3 g3

−g3 g1

p

dε1

p

dε3

(7.66)

Experimental results show that σ can be expressed by σ (s − s , κ) =

n Rρ −Aρ (s−s ) e , Aρ

ρ=1

© 2005 by Chapman & Hall/CRC Press

Aρ = Aρ (s, κ)

(7.67)

356

Continuum Mechanics and Plasticity

where Rρ and Aρ are material constants. Substituting (7.67) into (7.62) and neglecting terms of higher order of smallness, we obtain g1 =

3

Rρ Nρ e−Aρ (s−s ) ,

Nρ = cos θ − sin θ

ρ=1

g3 =

3

(κ + (dθ/ds)) Aρ (7.68)

Rρ Mρ e−Aρ

(s−s )

(κ + (dθ/ds)) Mρ = sin θ + cos θ Aρ

,

ρ=1

Substituting (7.68) into (7.66) and integrating the equation, yields 3 s σ1 −Aρ (s−s ) Nρ = Rρ e σ2 Mρ 0 ρ=1

−Mρ Nρ

p

dε1

p

dε3

(7.69)

This is the constitutive equation for a plastic strain trajectory. 7.5.2

The Endochronic Theory of Plasticity

The endochronic theory of plasticity was developed by Valanis [1] from the thermo-mechanical theory of internal variables. The theory will be discussed in detail in Chapter 8. The word endochronic is a Greek word for intrinsic time or internal time. Valanis introduced an intrinsic time ζ , which is monotonically increasing and is deﬁned by dζ 2 = Pijkm dεij dεkm

(7.70)

where Pijkm is a positive deﬁnite material tensor. In a special case, dζ may be deﬁned by the length of the strain path, that is, dζ 2 = dεij dεij

(7.71)

The constitutive equation has two parts, the deviatoric and volumetric part. They are σij

=2

ζ

ζ0

σkk = 3

ζ

ζ0

µ(ζ − ζ )

deij

dζ dζ

dεkk K(ζ − ζ ) dζ dζ

(7.72)

where µ(ζ ) and K(ζ ) are kernels of the integrals. In the one-dimensional stressing, (7.72) reduces to σ =

© 2005 by Chapman & Hall/CRC Press

ζ 0

E(ζ − ζ )

dε dζ

dζ

(7.73)

Advances in Plasticity

357

where E(ζ ) is a kernel function. Equations (7.72) and (7.73) are in the same form as (7.57), except that only the length of the strain path and not the curvature nor the torsion of the strain trajectory is included in the formulation. These geometrical parameters of the strain path may be accounted for by use of internal variables, and they have not been included for the sake of simplicity. It has been shown that using only the length of the strain path, the endochronic theory is capable of describing stress responses to complex strain paths. This version of endochronic theory is similar to but not quite the same as Ilyushin’s theory. One of the differences is in the deﬁnition of intrinsic time. The endochronic theory deﬁnes the intrinsic time by (7.70) using a material tensor Pijkm , whereas Ilyushin’s theory uses the arc length as the intrinsic time. Another difference, more signiﬁcantly, is that the endochronic theory is capable of accounting for volume change during deformation by use of the second equation of (7.72), while the theory of Ilyushin is formulated based on the deviatoric strain and no discussions have been given over to the volume change. It has been found that this version of endochronic theory does not correctly describe the unloading slope for metals and that it incorrectly predicts the same entropy production for further loading or unloading starting at a point already in the plastic state. Owing to the aforementioned deﬁciencies, an improved endochronic theory was developed by Valanis [2]. The new theory is free from the aforementioned deﬁciencies. In the new version, the intrinsic time is deﬁned by the plastic strain as p

p

dζ 2 = Pijkm dεij dεkm

(7.74)

The deviatoric part of the constitutive equation is σij

= 2G0

ζ 0

p

ρ(ζ − ζ )

dεij dζ

dζ

(7.75)

where G0 is a material constant and ρ(ζ ) is a kernel function. The volumetric change can be accounted for using the volumetric constitutive equation and the details of derivations are given in Chapter 8. It is shown in Chapter 8 that the ﬂow theory of plasticity may be derived from the new version of the endochronic theory. In addition, this theory is shown in Chapter 9 to apply to geotechnical materials which undergo plastic volume change during deformation.

7.6

Finite Plastic Deformation

Plastic deformations are large in cases such as metal forming, strain localization, ductile fracture, soil mechanics, and pavement analysis, etc. A plasticity

© 2005 by Chapman & Hall/CRC Press

358

Continuum Mechanics and Plasticity

theory of ﬁnite deformation must be used for these cases. The theories presented in previous sections of this chapter may be extended to the ﬁnite deformation range. The extension is not straightforward, however, and it has led to different opinions and heated debates. To extend an inﬁnitesimal theory into a ﬁnite theory, we encounter concepts such as the stress measure, the strain measure, the decomposition of strain into elastic and plastic parts, the objective rate (of stress, back stress, etc.), the observer independent yield function, and the rotation of material texture. The stress and strain measures and the decomposition of strain are discussed ﬁrst. The objective rate is then discussed in connection with hypoelasticity and discussion of its effects in plasticity is deferred until after a ﬁnite plasticity theory has been presented. Then the ﬁnite plastic simple shear deformation using different objective rates, and, ﬁnally, the yield function are discussed. 7.6.1

The Stress and Strain Measures

Either the Eulerian or the Lagrangian description may be used. The stress measures have already been discussed in Section 4.4.2.1 and strain measures in Sections 3.6, 3.9, and 3.10. In the Eulerian description, the stress and strains are referred to the current (deformed) conﬁguration. The Cauchy stress σ is usually used in this conﬁguration. This is the true stress, which is the force per unit deformed area. The Kirchhoff stress, which is deﬁned by Sij = Jσij where J is the Jacobian of the deformation equations, has also been used by some investigators. The Kirchhoff stress is also discussed in Chapter 11 in connection with the curvilinear coordinate system. Although we can use the Eulerian strain e or the left Cauchy–Green tensor B, it is more convenient to use the rate of deformation tensor D, which has the meaning of strain rate. The rate of deformation can be decomposed into the elastic and plastic parts and will be further discussed. In the Lagrangian description, the stress and strain refer to the undeformed (reference) conﬁguration. The nonsymmetric 1st P–K stress T(0) and the symmetric 2nd P–K stress have been used. Popular strain measures are the right Cauchy–Green tensor C and the Lagrangian strain (Green’s strain or Almansi strain) E. There is no uniﬁed approach available. The selection of the stress and strain measures greatly depends on the preference and convenience of the investigator and the problem at hand. 7.6.2

The Decomposition of Strain and Strain Rate

In the small deformation theory, it is customary to write p

εij = εije + εij

and

p

dεij = dεije + dεij

(7.76)

However, in ﬁnite deformation, the decomposition p

ERS = EeRS + ERS

© 2005 by Chapman & Hall/CRC Press

(7.77)

Advances in Plasticity

359

cannot be justiﬁed. This may be easily seen by considering the strain– displacement relation ERS

1 = 2

∂uR ∂uS ∂uk ∂uk + + ∂XS ∂XR ∂XR ∂XS

(7.78)

which cannot be separated into the sum of two parts because of the nonlinear terms in the displacement gradient. An additive decomposition was proposed by Green and Naghdi [56], who deﬁned Ee = E − Ep but explained that Ee was not an ordinary elastic strain tensor. It was deﬁned merely to represent the difference between the total strain E and the plastic strain Ep . The introduction of Ee was not necessary, because the use of E and Ep was sufﬁcient in their theory. On the other hand, the rate of deformation tensor can be separated into two parts because of the linear expression in the velocity gradient, that is, Dij = 12 (vi,j + vj,i )

(7.79)

p

It is possible to deﬁne two velocities vie and vi , such that Deij =

1 2

e e vi,j + vj,i

and

p

Dij =

1 2

p

p

vi,j + vj,i

(7.80)

Thus, p

Dij = Deij + Dij

(7.81)

We note that, in this connection, no attempt is made to separate the deformation gradient F into the elastic and plastic parts. In fact, F does not play a part in the formulation of (7.81). Another effort has been undertaken by researchers to derive the expressions of De and Dp starting from F. This effort involves some assumptions and physical justiﬁcations. Lee [57] introduced the concept of multiplicative decomposition of F. The deformation gradient has been previously discussed in Section 3.4. Let X express the initial conﬁguration of the body, x the elastic–plastic deformed state (the current conﬁguration), and p the state after de-stressing to zero stress. The deformation gradient F = ∂x/∂X with components FiR = ∂xi /∂XR expresses the total deformation. The deformation gradient Fp from the initial state X to the plastically deformed state p expresses the plastic deformation Fp =

© 2005 by Chapman & Hall/CRC Press

∂p ∂X

(7.82)

360

Continuum Mechanics and Plasticity

dx

F

X

x

dX

Fe

Fp dp

p X, x, p

FIGURE 7.23 Decomposition of F.

and Fe , from the plastically deformed conﬁguration p to x, expresses the elastic component of the deformation in the conﬁguration x, that is, Fe =

∂x ∂p

(7.83)

Thus, F = Fe · Fp

(7.84)

by the chain rule of differentiation. This decomposition of F into Fe and Fp is depicted by Figure 7.23. The intermediate conﬁguration p is obtained by an elastic de-stressing to zero stress from the current conﬁguration x and it represents a pure plastic deformation from X to p. If the plastic deformation is homogeneous, no residual stresses exist upon de-stressing and in this case Fe and Fp are continuous functions. However, if the plastic deformation is nonhomogeneous, residual stresses will result upon destressing. In order for all inﬁnitesimal material elements to reach a zero stress state, individual material elements will have to undergo a different amount of de-stressing. Therefore, in this case, Fe and Fp can be deﬁned as point-functions that relate the deformations in the inﬁnitesimal material elements. In addition, we mention that the intermediate state p is not uniquely deﬁned, because the elastic destressing can involve an arbitrary rigid-body rotation, which does not affect the stress. In order to have a unique p, we assume that the elastic de-stressing involves only pure deformation so that, by use of the polar decomposition of Section 3.5.2, the elastic part of the deformation gradient is Fe = Ve which is a symmetric tensor.

© 2005 by Chapman & Hall/CRC Press

(7.85)

Advances in Plasticity

361

Using (7.84) and (3.100), the Lagrangian strain is E = 12 (FT · F − 1) = 12 (FpT · FeT · Fe · Fp − 1) = 12 [FpT ·(FeT · Fe − 1)·Fp ] + 12 [FpT · Fp − 1] = FpT · Ee · Fp + Ep

(7.86)

where Ee = 12 (FeT · Fe − 1),

Ep = 12 (FpT · Fp − 1)

(7.87)

It is seen from (7.86) that the additive decomposition of Ee and Ep , as deﬁned here, does not hold, that is, E = Ee + Ep

(7.88)

The velocity gradient in the current conﬁguration x is L=

∂v ∂v ∂X = · = F˙ · F−1 ∂x ∂X ∂x

(7.89)

where F˙ is the material derivative of F. Substituting (7.84) into (7.89), we obtain −1 −1 −1 L = (Fe · Fp ) · (Fe · Fp )−1 = F˙ e · Fe + Fe · F˙ p · Fp · Fe

(7.90)

If we now choose the elastic de-stressing without rotation and the expression for Fe given by (7.85), and let −1 Lp = F˙ p · Fp = Dp + Wp

(7.91)

then ˙ e · Ve L=V

−1

+ V e · Dp · V e

−1

+ Ve · Wp · Ve

−1

(7.92)

From (7.92), the rate of deformation D and the spin tensor W take the form −1 −1 D = De + Ve · Dp · Ve S + Ve · Wp · Ve S −1 −1 W = We + Ve · Dp · Ve A + Ve · Wp · Ve A

(7.93)

where De , We (= 0, if Ve = VeT ), Dp , and Wp are the symmetric and antisym˙ e ·Ve−1 and Lp , respectively, and the subscripts S and A denote metric parts of V the symmetric and antisymmetric parts of a tensor. Looking at the expression for rate of deformation in (7.93), all three terms on the right-hand side of the equation are nonzero, in general. This indicates a very involved coupling of

© 2005 by Chapman & Hall/CRC Press

362

Continuum Mechanics and Plasticity

Ve , Dp , and Wp in combining to produce the total rate of deformation D. In this formulation, (7.92) cannot be reduced to the additive decomposition of D, expressed by (7.81), in the general case. However, elastic strain is small and negligible for most metals undergoing large plastic deformation, and we may use the approximation that Ve ≈ 1 to reduce (7.93) to D = De + Dp ,

W = We + Wp

(7.94)

On the other hand, Dafalias [58] introduced the concept of plastic spin based on Mandel’s concept of director vectors [59]. The plastic spin is a macroscopic representation of the rotation of material texture caused by plastic deformation. One way of observing the texture experimentally is to plot the pole ﬁgures. The rotation (or tilting) of texture has been observed experimentally by Montheillet et al. [60], Stout and O’Rourke [61], Toth et al. [62], and Wang et al. [63] in the torsion of thin-walled tubes or solid bars. Dafalias [64] further used the difference between the total spin W and the plastic spin Wp , termed constitutive spin ω to form the corotational rate. According to Dafalias, using Fe = Ve , (7.90) may be rewritten as ˙ e · Ve L=D+W =V = ω + Ve∇ · Ve

−1

−1

−1

+ Ve · F˙ p · Fp −1

+ Ve · Fp∇ · Fp

· Ve

· Ve

−1

−1

(7.95)

where the superscript ∇ denote the corotational rate, which has been discussed in Section 4.7.1. Since Ve transforms as a second-order tensor and Fp transforms as a vector upon the rotation of x (observer transformation), their corotational derivatives are ˙ e + Ve · ω − ω · Ve , Ve∇ = V

Fp∇ = F˙ p − ω · Fp

(7.96)

respectively. Restricting further to small elastic deformation for which Ve ≈ 1, the following are obtained from (7.95) −1

D = Ve∇ + (Fp∇ · Fp )S = De + Dp −1

W = ω + (Fp∇ · Fp )A = ω + Wp

(7.97)

with De = Ve∇ , rate of a symmetric elastic deformation; Dp and Wp the rates of plastic deformation and plastic spin, respectively. Thus, a portion of the total spin W is “absorbed” by the plastic spin and the rest accommodated by the constitutive spin ω. Dafalias [64] discussed the two deﬁnitions of “plastic spin” used in the literature and cautioned against deﬁning the plastic spin as the antisymmetric part of the velocity gradient at the plastically deforming intermediate conﬁguration. He suggested that the rotation of texture must be governed by a separate rule and not by the general kinematics of deformation. In the

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

363

continuum approach, constitutive equations must be provided not only for Dp but also for Wp , Mandel [59] and Kratochvil [65]. Dafalias writes Wp = λΩp (σ, s)

(7.98)

where λ is a parameter. An internal state variable s macroscopically describes the state of the microstructures. Using the representation theorem of Wang [66], Ωp can be represented by Ωp = η1 (s · σ − σ · s) + η2 (s · σ2 − σ2 · s) + η3 (σ · s · σ2 − σ2 · s · σ)

(7.99)

where η1 , η2 , and η3 are scalar valued functions of the invariants tr σ, tr σ2 , tr σ3 , tr(s · σ), and tr(s · σ2 ). Dafalias [64] and Loret [67] used the following simpliﬁed form to investigate the simple shear problem: Wp = η(α · σ − σ · α)

(7.100)

where η is a parameter and s is taken to be the back stress α. In addition, Dafalias [68] proposed the following form when he investigated plastic materials with kinematic hardening Wp = c(α · Dp − Dp · α)

(7.101)

where c is a parameter. EXAMPLE 7.1

Derive the corotational rate of vector g.

Solution Let g be subjected to an orthogonal transformation such that g¯ = QT · g

(a)

Dg¯ ˙ T · g + QT · g˙ =Q Dt

(b)

Then,

From the third equation of (4.92), we have ¯ = QT · W · Q + Q ˙ T · Q = QT · W · Q − Q T · Q ˙ W

(c)

˙ =W·Q−Q·W ¯ Q

(d)

or

© 2005 by Chapman & Hall/CRC Press

364

Continuum Mechanics and Plasticity

and ˙ T = QT · W T − W ¯ T · QT Q

(e)

Substituting (e) into (b), we obtain Dg¯ ¯ T · QT ) · g + QT · g˙ = (QT · WT − W Dt

(f)

¯ · g¯ = QT · (g˙ − W · g) g˙¯ − W

(g)

which leads to

It is to be noted that W is antisymmetric. The corotational rate of g can thus be deﬁned as ∇

g = g˙ − W · g

7.6.3

(h)

The Objective Rates

In Section 4.7 it was mentioned that only objective rates can be used to formulate a constitutive equation. There are many objective rates, however, and a reasonable objective rate should lead to results that can be veriﬁed by experiments. Different objective rates lead to different results and some are physically unacceptable results. For instance, it is known in hypoelasticity [69] that Jaumann rate gives rise to oscillatory shear and axial stresses with the increasing shear strain (see Section 4.10). In spite of this ﬁnding, some investigators continued to use the Jaumann rate in the ﬁnite deformation analysis. In the study of plasticity, Nagtegal and de Jong [70] analyzed the simple shear problem (shearing with constraint in axial direction) by use of the Jaumann rate for back stress using Prager’s linear kinematic-hardening rule. They showed an oscillatory shear stress response to monotonically increasing shear strain. This work triggered a series of investigations to look for objective stress rate appropriate for the description of metallic behavior in the ﬁnite strain range. Investigators have compared several objective stress rates with the purpose of eliminating the oscillatory stress–strain response. Yet, certain unreasonable behaviors, such as axial stress being zero or compressive with unacceptably large value, still exist in the available models. Furthermore, the majority of these models are for specimens subjected to loading only. When unloading or cyclic simple shearing are considered, the aforementioned unusual stress–strain behaviors can manifest itself in the unloading curve or the stress–strain loops. Discussions have been centered around two possibilities of eliminating the oscillatory behavior. One is to ﬁnd an objective rate that does not give rise to oscillatory stress responses even using a linear

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

365

constitutive equation. The other is to add a nonlinear term to the constitutive equation and, in this case, Jaumann rate does not lead to oscillatory stresses. In this subsection, the objective rate is discussed in connection with hypoelasticity. The effect of objective rate in plasticity is deferred to a later section. In the case of simple shear deformation, the hypoelastic constitutive equation is from (4.240) σij∗ = 2µDij

and

Dkk = 0

(7.102)

where σ∗ an objective rate and µ is the shear modulus. The simple shear deformation is governed by the following equations x1 = X1 + 2ωtX2 , u1 = 2ωtX2 ,

0 [L] = 0 0

0 0 , 0

2ω 0 0

x2 = X2 ,

u2 = u3 = 0,

0 [D] = sω 0

ω 0 0

x3 = X3

(7.103)

ω = const

(7.104)

0 0 , 0

0 [W ] = −ω 0

ω 0 0

0 0 0 (7.105)

The case of σ∗ equaling to the Jaumann rate σ∇ = (Dσ/Dt) − W · σ + σ · W has been discussed in Section 4.10. Following the procedures of Section 4.10, This section discusses the solutions of (7.102) and (7.105) using the Cotter–Rivlin stress rate [71], Oldroyd’s convected stress rate [72], the Green–McInnis rate [69], and the mixed objective stress rates. In the case of the Cotter–Rivlin stress rate, the stress rate is σ∗ =

Dσ + LT · σ + σ · L Dt

(7.106)

and the solution is σ11 = 0,

σ22 = −4µγ 2 ,

σ12 = 2µγ

(7.107)

where γ = 2ωt. Note that σ12 increases linearly and σ22 nonlinearly with γ . Even though the shear stress–strain curve does not oscillate, which satisﬁes the requirement, the magnitude of the axial stress is greater than that of the shear stress. According to the experimental ﬁndings of Montheillet et al. [60], White and Anand (reported in [73]), and Wu et al. [74], the magnitude of axial stress is about 10% of shear stress. The predicted high σ22 of this model makes the model unacceptable. In the case of Oldroyd’s rate, the stress rate is σ∗ =

© 2005 by Chapman & Hall/CRC Press

Dσ − L · σ − σ · LT Dt

(7.108)

366

Continuum Mechanics and Plasticity

On the other hand, Truesdell’s rate [75] is σ∗ =

Dσ + σ tr D − L · σ − σ · LT Dt

(7.109)

Since tr D = 0, (7.109) reduces to (7.108). The solution of this case is σ11 = 4µγ 2 ,

σ22 = 0,

σ12 = 2µγ

(7.110)

This model predicts a zero σ22 and a high magnitude of σ11 which are unacceptable for real materials. Using the Green–McInnis rate σ∗ =

Dσ − W∗ · σ + σ · W∗ Dt

˙ · RT where W∗ = R

(7.111)

in which tensor R is the orthogonal rotation tensor of the polar decomposition of the deformation gradient F, Dienes [69] obtained the following solution σ11 = −σ22 = 4µ[cos 2β ln(cos β) + β sin(2β) − sin2 β] σ12 = 2µ cos 2β[2β − 2 tan 2β ln(cos β) − tan β]

(7.112)

where tan β = ωt = 12 γ

(7.113)

The shear stress–strain curve of this model does not oscillate but the magnitude of axial stress is in the order of shear stress and does not agree with the experimental ﬁnding of approximately one-tenth of the magnitude of the shear stress. All the aforementioned solutions of hypoelasticity are plotted in Figure 7.24. EXAMPLE 7.2

Use the Green–McInnis rate to ﬁnd the stresses for simple

shearing. Solution The motion for simple shearing is from (3.20) x1 = X1 + 2X2 tan β,

© 2005 by Chapman & Hall/CRC Press

x2 = X2 ,

x3 = X3

(a)

Advances in Plasticity

367 Jaumann 22 = J22 Truesdell 22 = 0 Cotte–Rivlin 22 = C22 Dienes 22 = D22

Jaumann 12 = J12, Truesdell 12 = T12, Cotter–Rivlin 12 = C12, Dienes 12 = D12,

Stress MPa 60

C12, T12 D12

40 20

J12

–2

–4

4

2 D22

J22 C22

–60

FIGURE 7.24 Simple shear of hypoelastic material.

From (a), we ﬁnd

1 [F] = 0 0

2 tan β 1 0

0 0 , 1

1 2 T [U ] = [F] [F] = 2 tan β 0

0

[D] = sec2 β β˙ 0 2 tan β 0 4 tan2 β + 1 0 0 1

sec2 β β˙ 0 0

0 0 , 0

(b)

The eigenvalues and eigenvectors of [U 2 ] are λ2 = 1 + 2 tan2 β + 2 tan β sec β,

λ1 = 1,

λ3 = 1 + 2 tan2 β − 2 tan β sec β n1T = 0 n3T

0

1 ,

[(2 tan β − sec β) − 2 1] , n2T = (2 tan β − sec β)2 + 5

[(2 tan β + sec β) − 2 1] = (2 tan β + sec β)2 + 5

(c)

Therefore, [U] is

1

[U] = [n1

© 2005 by Chapman & Hall/CRC Press

n2

0

n3 ] 0

λ2

0

0

1/2

0

n1T

0 n2T 1/2 n3T λ3

(d)

368

Continuum Mechanics and Plasticity

We ﬁnd

[R] = [F][U]−1

cos β = − sin β 0

sin β cos β 0

0 0 , 1

sin β β˙ ˙ [R] = − cos β β˙ 0

cos β β˙ − sin β β˙ 0

0 0 0 (e)

and

0 T ˙ [w∗ ] = [R][R] = β˙ 0

β˙ 0 0

0 0 0

(f)

Using the Green–McInnis rate (7.111), the nonzero components of (7.102) are dσ11 ˙ 12 = 0 − 2βσ dt dσ12 ˙ 11 − σ22 ) = 2µ sec2 β β˙ + β(σ dt dσ22 ˙ 12 = 0 + 2βσ dt

(g) (h) (i)

Equations (g) to (i) are combined to yield d2 σ11 4µ + 4σ11 = dβ 2 cos2 β

with σ22 = −σ11

(j)

The general solution for (j) is σ11 = 4µ(cos 2β ln cos β + β sin 2β − sin2 β) + c1 cos 2β + c2 sin 2β

(k)

where c1 and c2 are constants and they vanish when all initial (at β = 0) stress components are zero. Substituting (k) into (g), gives (7.112).

7.6.4

A Theory of Finite Elastic–Plastic Deformation

The rate of deformation D is used in this section. According to the concept of work conjugate discussed in Section 4.4.3, the Cauchy stress σ is the work conjugate of D. An objective stress rate should be used and we use the Jaumann rate in this discussion. Other objective stress rates will be discussed in the next section. The Jaumann stress rate is σij∇ = σ˙ ij − Wip σpj + σip Wpj

© 2005 by Chapman & Hall/CRC Press

(7.114)

Advances in Plasticity

369

where σ˙ ij = Dσij /Dt. Denoting the deviatoric part of Dij by dij , we have p dij = dije + dij . The Mises yield criterion is f = ξijD ξijD −

2Y 2 =0 3

(7.115)

where ξijD = σij − αijD ; the superscript D denotes the deviatoric part of the quantity and Y is the current yield stress in tension. The plastic region is p characterized by f = 0 and dij dσij > 0, while the elastic region is characterized p

by either f < 0 or f = 0 and dij dσij ≤ 0. The tensor αij is the back stress. The elastic behavior is governed by σij ∇ = 2µdije

(7.116)

where µ is the shear modulus. The ﬂow rule is p dij = λ˙

∂f ∂σij

(7.117)

where λ˙ is a scalar factor of proportionality. Using (7.115), (7.117) reduces to p ˙ ijD dij = λξ

(7.118)

For simplicity, the linear isotropic-hardening rule is used and is written as Y˙ = βhd¯ p

(7.119)

where d¯ p is the equivalent plastic strain rate deﬁned by d¯ p =

p p 1/2 3 dij dij

2

(7.120)

and h is the slope of isotropic-hardening curve. The parameter β was previously discussed in (6.85) and β = 1 for isotropic hardening. Prager’s linear kinematic-hardening rule is used, that is, p

αijD∇ = 23 (1 − β)hdij

(7.121)

where β = 0 or kinematic hardening. The parameter β lies within 0 ≤ β ≤ 1. When β has a value between 0 and 1, then we have a combined isotropic– kinematic hardening.

© 2005 by Chapman & Hall/CRC Press

370

Continuum Mechanics and Plasticity

The factor λ˙ is determined from the consistency condition. Differentiating (7.115), gives 4Y ˙ f˙ = 2ξijD ξijD∇ − Y=0 3

(7.122)

The expressions in (7.122) can be shown as p ξijD ξijD∇ = ξijD σij ∇ − αijD∇ = ξijD 2µdije − 23 (1 − β)hdij = 2µdij ξijD − 2µ + 23 (1 − β)h λ˙ 23 Y 2 2 2 D D 1/2 2 ˙ 2 2 ¯p ˙ = 49 βhY 2 λ˙ 3 Y Y = 3 Yβhd = 3 Yβh 3 λ ξij ξij

(7.123)

By substituting the two expressions of (7.123) into (7.122), we obtain 2µdij ξijD = 23 λ˙ Y 2 2µ + 23 (1 − β)h + 23 βh

(7.124)

which may be solved for λ˙ to obtain λ˙ =

dij ξijD 3 2 Y 2 (1 + (h/3µ))

(7.125)

˙ the rate of deformation may now be Having found the expression for λ, written as p

dij = dije + dij =

σij ∇ 2µ

+

D D 3 dkm ξkm ξij 2 Y 2 (1 + h/3µ)

(7.126)

This equation may be inverted to obtain σij ∇

= 2µ δik δjm −

D ξD ξkm ij

(2/3)Y 2 (1 + h/3µ)

dkm

(7.127)

that is, the stress rate is expressed in terms of the rate of deformation dij . This equation is often written as σij ∇ = Lijkm dkm

(7.128)

to facilitate computation. We note that the volumetric behavior is assumed to be elastic which is described by 1 ˙ kk 3σ

where K is the bulk modulus.

© 2005 by Chapman & Hall/CRC Press

= KDkk

(7.129)

Advances in Plasticity

371

Using the theory of this section to derive the stress–strain relation for uniaxial stress.

EXAMPLE 7.3

Solution In the case of uniaxial stress 2 0 0 3σ σ

[σ ] = 0 0 −3 , σ 0 0 − 3 2α 0 0 3 α [α D ] = 0 − 0 3 α 0 0 3

ε˙ p

[Dp ] = [dp ] = 0 0

0 1 p − ε˙ 2 0

0

0 1 p − ε˙ 2

(a)

Using (a), the yield function (7.115) is reduced to σ =Y+α

(b)

and, using (7.125), the equivalent plastic strain rate is d¯ p = { 23 [(˙ε p )2 + 2(− 12 ε˙ p )2 ]}1/2 = ε˙ p

(c)

The linear isotropic-hardening rule is then given by Y˙ = βh˙εp

(d)

and the linear kinematic-hardening rule is from (7.121) and (7.130) reduces to α˙ = (1 − β)h˙ε p

(e)

˙ and αD∇ = α˙ D . The expression for (d) is the We note that due to W=0, σ∇ = σ, same as (6.147) and the expression for (e) is the same as (6.149). The roles of isotropic and kinematic hardening are similar to those shown in Figure 6.21(b). Using (d) and (e), the stress–plastic strain curve is given by σ˙ = Y˙ + α˙ = βh˙εp + (1 − β)h˙ε p = h˙εp

(f)

The slope of the stress–plastic strain curve may be identiﬁed as h=

© 2005 by Chapman & Hall/CRC Press

σ˙ dσ = p ε˙ p dε

(g)

372

Continuum Mechanics and Plasticity

where the slope is a function of ε p . The total strain is σ˙ σ˙ ε˙ = ε˙ + ε˙ = + = E h e

p

1 1 + σ˙ E h

(h)

where E is the elastic modulus. In the stress–strain curve, the slope is 1 dσ = = Et dε (1/E) + (1/h)

(i)

where Et is the tangent modulus. Therefore, Et =

hE h+E

(j)

This equation relates Et to E and h. Using (i), the axial stress–strain curve may be plotted. It is noted that the ﬂow rule is not explicitly used in this one-dimensional case. A rectangular metal block with edges parallel to the x, y, z-axes is compressed in the x-direction between overlapping rigid plates. Expansion is allowed only in the y-direction, and is prevented in the z-direction by rigid dies. All contact surfaces are perfectly lubricated so that the deformation is plane and uniform. The compressive strain in the x-direction is controlled and it increases monotonically from zero. Determine the stresses. Use the theory of this section and assume that the material hardens only by isotropic hardening.

EXAMPLE 7.4

Solution Assume that in the elastic region, the behavior is hypoelastic so that p σ˙ ij = λδij Dkk + 2µ Dij − Dij

with Dkk = Dekk

(a)

We note that since W = 0 for this problem, σij∇ = σ˙ ij . The ﬂow rule is ˙ ij

Dij = φσ p

p

(b)

p

where Dij = dij due to plastic incompressibility. Parameter φ is used here so that a distinction can be made between this parameter and the Lamé constant λ used in (a). The equivalent plastic strain rate is ¯p = D

© 2005 by Chapman & Hall/CRC Press

p p 1/2 3 Dij Dij

2

(c)

Advances in Plasticity

373

and the yield function is 2Y 2 =0 3

f = σij σij −

(d)

with the consistency condition 4Y ˙ f˙ = 2σij σ˙ ij − Y=0 3

(e)

The isotropic hardening is ¯ p, Y˙ = hD

β=1

(f)

Dij σij

3 2 Y 2 (1 + h/3µ)

(g)

Using (7.125), we obtain φ˙ =

Substituting (g) and (b) into (a), we ﬁnd

σij

σ˙ ij = λδij Dkk + 2µDij − BDkm σkm

(h)

where B=

3µ Y 2 (1 + h/3µ)

(i)

The boundary conditions are σx = 0,

σy = 0,

σz = 0,

Dx = 0 (known),

Dy = 0, Dz = 0 (j)

Apply the conditions σ˙ y = 0 and Dz = 0 in (h) gives Dy = −

C1 Dx C2

(k1)

where

© 2005 by Chapman & Hall/CRC Press

C1 = 3λ + B(σx + σz )(2σx − σz )

(k2)

C2 = 3λ + 6µ − B(σx + σz )2

(k3)

374

Continuum Mechanics and Plasticity

The other two components of (h) are σ˙ x = λ(Dx + Dy ) + 2µDx − A(2σx − σz )

(l1)

σ˙ z = λ(Dx + Dy ) − A(2σz − σx )

(l2)

where A=

−1 σx + σ z

[λ(Dx + Dy ) + 2µDy ]

(l3)

and (k1) was used in the derivation of (l3). Equations (l1) to (l3) can be further reduced to σ˙ x = C3 Dx + C4 Dy

(m1)

σ˙ z = C5 Dx + C6 Dy

(m2)

where

3σx C3 = 2µ + λ σx + σ z 3σz C5 = λ , σx + σ z

σx − 2σz , C4 = C3 + 2µ σx + σ z σx − 2σz C6 = C5 − 2µ σx + σ z

(m3)

Finally, we substitute (k1) into (m1) and (m2) to obtain

C 1 C4 σ˙ x = C3 − C2

Dx

and

C 1 C6 σ˙ z = C5 − C2

Dx

(n)

It is to be noted that Ci are functions of σx , σz and material constants. If we know Dx , then σx and σz may be calculated by the integration of (n), and Dy may be found from (k1). Additional exercises may be performed by plotting the σx versus Dx dt and σz versus Dx dt curves. In addition, Dy may be plotted as a function of Dx and the effect of h on the results discussed. An experimental study of the biaxial compression problem was conducted by Khan and Wang [76].

7.6.5

A Study of Simple Shear Using Rigid-Plastic Equations with Linear Kinematic Hardening

The subject of study in this section is the problem of simple shear using rigid-plastic equations with linear kinematic hardening, that is, β = 0. Three objective rates are considered. They are the Jaumann rate, the Dafalias rate, and Lee’s rate [77].

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

375

7.6.5.1 The Jaumann rate The Mises yield criterion is 3

2 (σ

− αD ) · (σ − αD ) = Y 2

(7.130)

The kinematic-hardening rule is from (7.121) αijD∇ = 23 hDij

(7.131)

p

where dij = dij = Dij and Dkk = 0. The Jaumann rate is given by (7.114) and the ﬂow rule is from (7.118) Dij = λ˙ σij − αijD

(7.132)

Using the ﬁnite simple shear straining described by (7.105), we obtain from (7.132)

D σ11 = α11 ,

D σ22 = α22 ,

D σ12 = α12 +

ω Y D +√ = α12 λ˙ 3

(7.133)

The last expression was obtained using (7.132) and (7.130). The expression of (7.131) is in the form of (7.102), whose solution in the case of Jaumann rate is given by (4.248). Therefore, the solution for (7.131) is D α12 =

h sin γ , 3

D D = −α22 = α11

h (1 − cos γ ) 3

(7.134)

D + α D = 0 and, therefore, from the ﬁrst two From (7.134) we infer that α11 22

= −σ or (2σ − σ )/3 = −(2σ − σ )/3. equations of (7.133) we obtain σ22 22 11 11 22 11 Thus, σ11 + σ22 = 0 or σkk = 0, since σ33 = 0. Using this result, we conclude

and σ = σ . Equations (7.133) and (7.134) combine to yield that σ11 = σ11 22 22

Y h σ12 = √ + sin γ , 3 3

σ11 = −σ22 =

h (1 − cos γ ), 3

other σij = 0 (7.135)

This is the solution for the simple shear problem by use of the Jaumann rate for the back stress. It is seen that all nonzero stress components are oscillatory. Finally, it is easy to show that by eliminating γ from the equations of (7.134), we ﬁnd

D α12

2

+

h D − α11 3

2

=

2 h 3

(7.136)

that is, the back stress is making a circular motion when the Jaumann rate is used.

© 2005 by Chapman & Hall/CRC Press

376

Continuum Mechanics and Plasticity

7.6.5.2 The Dafalias rate The yield function is given by (7.130) and the ﬂow rule is given by (7.132). Upon the substitution of (7.105) into (7.132), we obtain (7.133). The kinematichardening rule is ∗

αijD = 23 hDij

(7.137)

in which ∗

αijD =

DαijD Dt

− ωij αjiD + αijD ωji

(7.138)

is the Dafalias rate; ωij is the constitutive spin deﬁned by (7.97) and is written as p ωij = Wij − Wij = Wij − η αijD Dji − Dij αjiD

(7.139)

where η is a parameter which describes the strength of plastic spin. By use of (7.105), it is easily shown that

0 [ω] = ξ −ω 0

0 0 0

ω 0 0

D D with ξ = 1 − η α11 − α22

(7.140)

Thus, (7.137) is reduced to

D α11

D α D Dt 12 0

D α12 D α22

0

0

D 2α12

D D 0 − ξ ω α22 − α11 0 0

D − αD α22 11 D −2α12

0

0 0 2 ω h = 0 3 0 0

ω 0 0

0 0 0

(7.141) The nonzero components of the equation are D Dα11 D D D 1 − ηα11 ω + ηα22 = 2α12 Dt D Dα22 D D D 1 − ηα11 ω + ηα22 = −2α12 Dt D D Dα12 2 D D D 1 − ηα11 ω − α11 + ηα22 = hω + α22 3 Dt

© 2005 by Chapman & Hall/CRC Press

(7.142)

Advances in Plasticity

377

D = α D = 0 initially, α D = −α D for all t. Using this result, (7.142) is Since α11 22 11 22 simpliﬁed to yield D D dα11 D α12 , = 1 − 2ηα11 dγ

D D dα12 h D α11 = − 1 − 2ηα11 dγ 3

(7.143)

D /Y and where γ = 2ωt. We now introduce dimensionless variables αˆ 11 = α11 D αˆ 12 = α12 /Y, and a parameter hˆ = h/(3Y), so that (7.143) may be written as

dαˆ 11 ˆ αˆ 11 )αˆ 12 , = (1 − hρ dγ

dαˆ 12 ˆ αˆ 11 )αˆ 11 = hˆ − (1 − hρ dγ

(7.144)

where ˆ = 2ηY hρ

(7.145)

The equations in (7.143) are solved numerically by Dafalias [58]. The boundary condition is αijD = 0 at initial yielding. Similar to (7.133), we may establish that D σ11 = α11 ,

D D σ22 = α22 = −α11 ,

Y D σ12 = α12 +√ 3

(7.146)

In Figure 7.25(a), we plot the shear stress–strain curves with values of hˆ = 1.0, 1.5, 1.6, 1.7, 1.75, and 2.0, while keeping ρ = 0.08. The corresponding axial stress versus shear strain curves are plotted in Figure 7.25(b), and the corresponding back stress paths as the shear strain γ increases are plotted in Figure 7.25(c). It clearly shows that the solution is very sensitive to the relative value between hˆ and ρ. A large ρ indicates a strong plastic spin and the corresponding constitutive spin is small. When hˆ is relatively small such as 1.0, the constitutive spin is signiﬁcant and it causes the back stress to spin as indicated in Figure 7.25(c). As a result, both the axial and shear stresses are ˆ but they are very oscillatory. The stresses are not oscillatory for larger h, sensitive to this parameter as seen from Figure 7.25(b) and (c). We would also like to mention that generally the magnitude of axial stress of this model is larger than the shear stress, which is not reasonable. 7.6.5.3

The rate of Lee

Lee et al. [77] proposed a spin W∗ to replace the spin tensor W in the Jaumann rate, achieving nonoscillatory stresses in simple shearing. The tensor W∗ is determined by the angular velocity of the material line element which is instantaneously coincident with the eigenvector associated with the maximum eigenvalue of back stress α. The spin W∗ is expressed by Wij∗ = Wij + Dik nk nj − ni nk Dkj

© 2005 by Chapman & Hall/CRC Press

(7.147)

378

Continuum Mechanics and Plasticity (a)

4

5

2.0

1.7

7

1.

12 /Y

3 2

1.0

1.6

1 2

6

4

8

10

–1 15 –2 (b)

6

1.7

1.75

1.6

5 0

2.

11/Y

4

1.

5

3 2

1.

0

1 2

–1

4

6

8

10

–2 (c) 2.0

12.5

12 /Y

10 1.75

7.5 5

1.7

2.5 1

1.0 3

5

1.6 /Y 7 11

1.5 FIGURE 7.25 Simple shear using Dafalias’s rate: (a) shear stress–strain curves, (b) axial stress, (c) back stress.

where n is that eigenvector of α. Lee et al. [77] pointed out that kinematic hardening is an anisotropic phenomenon for which speciﬁc directions embedded in the material and the rotation of these particular directions play a signiﬁcant role. It is noted, however, that the rotation of the eigenvector used to deﬁne W∗ is a part of the kinematics of deformation and is not directly related to the rotation of the material texture. Dafalias rate is different

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

379

in that it contains a parameter that is related to the spin of the material texture. Following [77], we now use W∗ in connection with the corotational rate to investigate the simple shear deformation. The rate of Lee et al. may be written as ∗

αD =

DαD − W ∗ · αD + α D · W ∗ Dt

(7.148)

Since a corotational rate is objective, Lee’s rate is objective. For the simple shear deformation deﬁned by (7.105), the line element associated with W∗ is on the (x1 , x2 ) plane. Thus, [n]T = [n1 n2 0]. Substituting this expression of [n] into (7.147), we ﬁnd

1 0 0 0 0 0

0 [W ∗ ] = 2n22 ω −1 0

with n21 + n22 = 1

(7.149)

Using (7.149) and (7.148), the nonzero components of the linear kinematichardening rule (7.137) are D D α˙ 11 − 4n22 ωα12 =0 D D α˙ 22 + 4n22 ωα12 =0

(7.150)

D 2h D D α˙ 12 − 2n22 ω α22 − α11 = ω 3 Equations in (7.150) are further reduced to D = α˙ 12

2h D ω − 4n22 ωα11 , 3

D D α˙ 11 − 4n22 ωα12 = 0,

D D and α22 = −α11

(7.151)

We now determine the eigenvector n. We have

D −λ α11

D α12 0

0 n1 0 n2 = 0 0 0 0−λ

D α12

0

D −λ α22

0

(7.152)

From (7.152), we obtain n1 = 1 − n22 ,

n2 =

1 R2 + 1

,

R=

D + −α22

D α22

2

D 2 + α12

D α12

(7.153)

© 2005 by Chapman & Hall/CRC Press

380

Continuum Mechanics and Plasticity 2.0

(a)

1.5

12/ Y

6

1.0

4 2

2

4

8

6

(b) 12

2.0

10

1.5

8 11/Y

10

6

1.0

4 2

2 (c)

4

8

6

10

7

2.0

6 12/Y

5

1.5

4

1.0

3 2 1

2

4

6

11/Y

8

10

12

FIGURE 7.26 Simple shear using Lee’s rate: (a) shear stress–strain curves, (b) axial stress, (c) back stress.

The positive n2 is chosen which corresponds to the maximum eigenvalue. D and α D . Knowing In this way, n2 is expressed in terms of components α22 12 D αij , we determine [n], which may then be substituted into (7.151). Finally, we mention that (7.146) still applies in this case. Numerical results for simple shear using Lee’s rate are plotted in Figure 7.26(a) to (c). The curves are plotted for hˆ = 1.0, 1.5, and 2.0. We see that all curves are not oscillatory, but the predicted axial stress is too large.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity EXAMPLE 7.5

381

Show that W∗ of Lee’s rate represents the spin of a material

line element. Solution Let the line element be dxi and be denoted by dxi = ni ds

(a)

where ni is the unit vector along the line element and ds is the length of the line element. The relative velocity between the ends of the line element is dvi =

∂vi dxj = Lij nj ds ∂xj

(b)

The component of dv normal to n determines the spin W* of that line element to within an arbitrary spin. The component of dv normal to n is denoted by dv∗ = dv − (dv · n)n

(c)

Then, (c) in the subscript notation is dvi∗ = dvi − dvk nk ni = Lij nj ds − Lkj nj dsnk ni = (Dij + Wij )nj ds − (Dkj + Wkj )nj nk ni ds = Dij nj ds + Wij nj ds − Dkj nj nk ni ds

(d)

dv∗ = w∗ × n ds

(e)

But,

where w∗ is the dual vector of W∗ . In the index notation, (e) is dvi∗ = eijk wj∗ nk ds = ekij wj∗ nk ds = −Wki∗ nk ds = Wik∗ nk ds

(f)

Equating (d) and (f), we obtain Wik∗ nk = Dij nj (nk nk ) + Wij nj − Dkj nj nk ni

(g)

Wij∗ = Wij + Dik nk nj − ni nk Dkj

(h)

which reduces to

© 2005 by Chapman & Hall/CRC Press

382

Continuum Mechanics and Plasticity

EXAMPLE 7.6

Let the simple shear motion be

0 [D] = ω 0

ω 0 0

0 0 , 0

0 [W ] = −ω 0

ω 0 0

0 0 0

(a)

Find the expression of [W*]. Solution Let [n] = (cos θ , sin θ , 0), then from (7.147)

0 [W ∗ ] = −2ω sin2 θ 0

0 0 0

2ω sin2 θ 0 0

(b)

Since wk∗ = − 12 eijk Wij∗

(c)

We ﬁnd [w∗ ]T = 0

0

−2ω sin2 θ

(d)

Thus, the angular velocity w3∗ = θ˙ of the line element varies with the direction of the line element deﬁned by angle θ . The line along the x1 -axis does not rotate and the spin is maximum along the x2 -axis. 7.6.5.4

Remarks about objective rates of plasticity

The spin W is overemphasized by the Jaumann rate. In simple shear, W is the angular velocity θ˙ of the line element, along the principal direction of D, making a θ = π/4 angle with the x1 -axis. Referring to Figure 7.27, a square material element initially at OA0 B0 C assumes the shape OABC during simple shearing. As the shear strain becomes large, all lines emanating from O and lying within the angle ∠AOC have small angles θ, which are less than π/4. According to Lee et al. [77], these lines do not have the same θ˙ and do not rotate much. The line along OC does not spin at all and the line along OA does not spin as much as W. This effect may be seen from Example 7.5 by using a small θ in equation (d). It is noted that both Dij and Wij refer to a square element, with sides parallel to the x1 and x2 axes, deﬁned at the current conﬁguration. Therefore, W represents the spin of this new element which does not contain the same material mass as the original element. The Jaumann rate overemphasizes W because it does not represent the spin of the original material element.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

383

x2

1

A0

0

B0

C

A

B

x1

FIGURE 7.27 Rotation of line element during simple shearing.

From the discussions of previous subsections, we see that some objective rates lead to oscillatory stress components in simple shearing when the shear strain is monotonically increasing. This effect is of course in violation of experimental observations. Of the several objective rates discussed none can lead to acceptable stress responses using a linear kinematic-hardening equation. Several rates lead to an axial stress which is about the same or larger in magnitude than the shear stress, while experimental results show that the axial stress is about one-tenth of the magnitude of the shear stress. A conclusion may be drawn that these rates will have to be applied to a nonlinear kinematic-hardening equation. The concept of constitutive spin proposed by Dafalias [64] is promising. It introduces a constitutive equation for the plastic spin which is a macroscopic description of the spin of material texture. From the experimental investigation of material textures [60–63], it is known that the spin (or tilting) of the material texture is not directly expressed by the general kinematics of deformation. In the case of torsion, for instance, a monotonic increasing shear deformation can cause the texture to rotate in a direction of decreasing shear strain and then reverse its direction as the shear strain becomes larger. This is the evidence that plastic spin should not be deﬁned by the general kinematics of deformation. The plastic deformation induced anisotropy is described to a large extent by the kinematic hardening. Since plastic deformation changes the material texture, it is reasonable to use the back stress to describe the texture rotation. As previously mentioned, the plastic spin is independent of the kinematics of deformation, while the stress rate and the strain rate are dependent of the same. Therefore, different objective rates should be used for back stress, stress, and strain. In Wu [78,79], we use Dafalias rate for the back stress, and the convected rate for the stress and strain. This approach will be further discussed in Chapter 11 in connection with a curvilinear coordinate system.

© 2005 by Chapman & Hall/CRC Press

384 7.6.6

Continuum Mechanics and Plasticity The Yield Criterion for Finite Plasticity

Most works of ﬁnite plasticity have focused on the decomposition of deformation into elastic and plastic parts and the objective stress rates or back stress rates. Little attention has been given to the yield criterion applicable in the ﬁnite deformation range. Most theoretical works have assumed that the Mises yield criterion can be used. Some apply the Mises criterion expressed in terms of the Cauchy stress and some the 2nd P–K stress. The main concern is that yield criterion should be observer independent. For an isotropic material, this statement is equivalent to the requirement that the yield criterion be independent of rigid-body rotation of the material element. However, this is only an approximation because the material does not remain isotropic during plastic deformation. A yield criterion is observer independent, if it is deﬁned by stress invariants. It is noted, however, that a square material element used to deﬁne the Cauchy stress does not remain square during plastic deformation. If referring to the orientation of another observer, a square element is chosen to describe the state of stress, the aforementioned two square elements do not contain the same material mass. The two elements can be compared only when material isotropy is assumed and the concept of stress invariants is based on this assumption. In Chapter 11, an observer independent yield criterion will be deﬁned in terms of the contravariant true stress, which remains unchanged either during an observer transformation or when the material element undergoes a superimposed rigid-body rotation. In the remainder of this section, we investigate the effect of stress measure on the shape, size, and translation of the yield surface when the specimen has been prestrained into the ﬁnite deformation range. Speciﬁcally, we compare the yield surfaces in the combined axial–torsion problem when the yield function is deﬁned by the Cauchy stress, the 1st P–K stress, and the 2nd P–K stress, following the study of Wu et al. [24]. Usually, the stresses in the experimental data are the physical components in the cylindrical-coordinates system, so that all stress components have the same unit. The physical components will be discussed in Chapter 11 in connection with the curvilinear coordinates. The physical components in the present case are components of a tensor referred to unit vectors er , eθ , ez in the radial, tangential, and axial direction, respectively. Determine the physical components of the deformation gradient F in the cylindrical coordinate system.

EXAMPLE 7.7

Solution Let (r, θ , z) be the cylindrical coordinates of a point having Cartesian coordinates (x, y, z). The following equations hold x = r cos θ ,

© 2005 by Chapman & Hall/CRC Press

y = r sin θ,

z=z

(a)

Advances in Plasticity

385

An inversion of (a) yields r 2 = x2 + y 2 ,

θ = tan−1

y x

z=z

,

(b)

The unit base vectors of the cylindrical system are (er , eθ , ez ), and the unit vectors of the Cartesian system are (ex , ey , ez ). These unit vectors are related by er = cos θex + sin θey ,

eθ = − sin θex + cos θey

(c)

Taking the partial derivatives of (b) and using (a), we obtain ∂r x = = cos θ, ∂x r

∂r y = = sin θ, ∂y r

∂θ −y −y − sin θ = 2 = 2 = , 2 ∂x r x +y r

∂θ cos θ = ∂y r

(d)

Differentiation of (c) gives ∂eθ ∂ez ∂ez ∂er ∂eθ ∂ez ∂er = = = = = = =0 ∂r ∂r ∂r ∂θ ∂z ∂z ∂z ∂eθ ∂er = eθ , = −er ∂θ ∂θ

(e)

Consider now the undeformed position vector P and the current position vector p of a point expressed in the cylindrical system as P = ReR + ZeZ ,

p = rer + zez

(f)

where (R, Z) and (r, z) are components of the undeformed and deformed position vectors, respectively; (eR , eZ ) and (er , ez ) are the unit vectors of the two systems. Using (e), the differential forms for (f) are dP = dReR + R de + dZeZ ,

dp = drer + rdθeθ + dzez

(g)

We now proceed to ﬁnd a relation between the components of dp and those of dP. To this end, we note that r, θ, z are functions of R, , Z. Thus, by chain rule of differentiation, we obtain ∂r ∂r ∂r dR + R d + dZ ∂R R∂ ∂Z r∂θ r∂θ r∂θ dR + Rd + dZ r dθ = ∂R R∂ ∂Z ∂z ∂z ∂z dz = dR + Rd + dZ ∂R R∂ ∂Z dr =

© 2005 by Chapman & Hall/CRC Press

(h)

386

Continuum Mechanics and Plasticity

Using (h), the components of (g) may be written in matrices as

∂r ∂R dr r∂θ [dp] = r dθ = ∂R dz ∂z ∂R

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂Z dR r∂θ R d = [F][dP] ∂Z dZ ∂z ∂Z

(i)

where the components of the deformation gradient are

∂r ∂R r∂θ [F] = ∂R ∂z ∂R

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂Z r∂θ ∂Z ∂z

(j)

∂Z

7.6.6.1 Relations among stress measures for thin-walled tubes The text of this section was originally presented in [24]. Considering the axial– torsion of a thin-walled tube, two sets of cylindrical coordinates (X 1 , X 2 , X 3 ) = (R, , Z) and (x1 , x2 , x3 ) = (r, θ, z) are used to describe the undeformed and deformed status, respectively. The two sets of coordinates are related by r = λm Rm − λ2 (Rm − R) = (λm − λ2 )Rm + λ2 R θ = + ϕλ3 Z

(7.154)

z = λ3 Z in the range of R1 ≥ R ≥ R0 , where R1 and R0 are the undeformed outer and inner radii, respectively; and r1 ≥ r ≥ r0 , where r1 and r0 are the deformed outer and inner radius, respectively; λm = rm /Rm describes the stretch ratio of the mean radii which are denoted by Rm and rm in the undeformed and deformed status, respectively; λ2 = h/H describes the stretch ratio of the wallthicknesses, which are denoted by H and h in the undeformed and deformed status, respectively; λ3 = z/Z describes the deformation in the axial direction, which is denoted by Z and z in the undeformed and deformed status, respectively; and ϕ is the angle of twist per unit deformed length and is related to the shear strain γ by γ = rϕ

(7.155)

We note that if the value of λi (i = m, 2, 3) is greater than one, then it implies stretching; if it is equal to one, then there is no length change; and there is contraction when this value is less than one. Taylor and Quinney [9] found

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

387

that the hoop and radial strains are not equal for a thin-walled tube under combined tension–torsion loading condition. According to Taylor and Quinney, the values of λm and λ2 are the same for the tension only condition but are different and depend on the constitutive equations used for the combined tension–torsion loading condition. It has been shown in Example 7.6 that the physical components of deformation gradient F are

∂r ∂Z r∂θ ∂Z ∂z

∂r R∂ r∂θ R∂ ∂z R∂

∂r ∂R r∂θ [F] = ∂R ∂z ∂R

(7.156)

∂Z

Using (7.154), (7.156) reduces to

λ2

[F] = 0 0

λ2 0 = ϕλ3 r 0 λ3

0 r R 0

0

0 λm 0

0 γ λ3 λ3

(7.157)

The last expression of (7.157) is found by considering the mean radius of the tube, where R = Rm , r = rm = λm Rm and γ = rm ϕ. The inverse of the above matrix is

λ−1 2

[F]−1 = 0 0

0

0

λ−1 m

−Rm ϕ

(7.158)

λ−1 3

0

When the material is incompressible, which is a reasonable assumption for metallic materials undergoing large plastic deformation, the Jacobian is J = β2 β3 βm = 1

(7.159)

We now proceed to ﬁnd the relations among the components of Cauchy stress σ, 1st P–K stress T(0) , and 2nd P–K stress . These relations have been previously discussed in Section 4.4.2.1, and the equations are from (4.42) and (4.50) σ = J −1 F · T(0)

and

= T(0) · F−T

(7.160)

For the case of thin-walled tube under axial–torsional loading condition, the stress states of σ, T(0) , and are given by their respective physical

© 2005 by Chapman & Hall/CRC Press

388

Continuum Mechanics and Plasticity

components as

0 [σ ] = 0 0

0 0 τ

0 τ, σ

0 (0) [T ] = 0 0

0 T θθ T zθ

0 T θz , T zz

0 [] = 0 0

0 θθ zθ

0 θz zz (7.161)

in which σ zz = σ is the axial stress which is equal to the axial force divided by 2πrm h; σ θz = σ zθ = τ is the shear stress, which is equal to the torque divided 2 h; σ θθ = 0 due to symmetry and σ rr = 0 due to no surface tractions by 2π rm on both the inner and outer lateral surfaces of the tube. The last condition is an approximation, but it is justiﬁable when the wall is thin. Substituting (7.157) to (7.159) and (7.161) into (7.160), we obtain 0 0 0 [σ ] = 0 λm T θθ + ϕRm λm λ3 T zθ λm T θz + ϕRm λm λ3 T zz 0 λ3 T zθ λ3 T zz 0 0 0 1 0 −τ Rm ϕ (τ − ϕRm λm σ ) [T (0) ] = λm τ σ 0 λ3 λ3 0 0 0 T θz 0 1 T θθ − ϕRm λm T θz [] = λm λ3 T zz 1 zθ zz 0 T − ϕRm λm T λm λ3

(7.162)

(7.163)

(7.164)

The component T zθ , which equals the torque divided by 2π Rm Hrm , and the component T zz , which equals the axial force divided by 2π Rm H, are known quantities from experiment, where Rm is the mean radius of the tube in the undeformed conﬁguration and an approximated rm may be obtained by measuring the deformed outer radius r1 and then subtracting H/2 from it. For convenience, most experimental results in the literatures are presented in terms of the 1st P–K stress components T zz and T zθ . However, this is only an approximation since rm is not measured in most experiments. The current wall-thickness h is very difﬁcult to measure. The other components of T(0) cannot be readily determined experimentally in the case considered. However, they may be expressed in terms of T zz and T zθ . To this end, we obtain, from (7.161) and (7.162), the following relations σ θθ = 0 = λm T θθ + ϕRm λm λ3 T zθ σ

© 2005 by Chapman & Hall/CRC Press

θz

= τ = λm T

θz

+ ϕRm λm λ3 T

zz

(7.165) (7.166)

Advances in Plasticity

389 σ zθ = τ = λ3 T zθ σ

zz

(7.167)

zz

(7.168)

T θθ = −ϕRm λ3 T zθ

(7.169)

= σ = λ3 T

From (7.165), we obtain

and, by substituting (7.167) into (7.166), we have T θz =

1 λ3 T zθ − ϕRm λm λ3 T zz λm

(7.170)

Thus, all components of the 1st P–K stress may be determined. By using (7.167) and (7.168), Cauchy stress components may be calculated. In view of (7.161), the state of Cauchy stress can be completely determined. It is seen that when the axial strain is equal to zero, that is, λ3 = 1, we have σ zθ = T zθ and σ zz = T zz . But if the axial strain is large, then the difference between the two measures can be large. These transformation equations are used in the next section where theoretical predictions of yield surfaces are compared with experimental data. For the axial prestrain only condition, we have λm equaling λ2 [9]. From (7.159), we then obtain the relations among λi as λm = λ2 =

1 λ3

(7.171)

For the torsional prestrain only condition, all values of λi ’s may be approximated by one. This may be estimated by use of experimental results of Wu and Xu [80] for pure torsion of 304 stainless steel. It has been found that for an angle of relative grip rotation of 32.5◦ , ϕ is 12.76 rad/m and the corresponding engineering shear strain is 10.3%, which gives rise to an axial strain ε of 0.23%. Using (7.154), we found that λ3 = 1.0023 which may be approximated by 1 in this case. Since the diameter of the thin-walled tube undergoes a small amount of change during pure torsion, we obtain the following approximated relations among λi , that is, λm ∼ = λ2 ∼ = λ3 ∼ = 1. These relations are used in the next section and are further discussed. 7.6.6.2 Experimental determination of yield surfaces Experiments were conducted, by use of a computer-controlled, axial– torsional, closed-looped, electrohydraulic materials test system. The same batch of annealed 304 stainless steel specimens as in Wu and Yeh [4] was used in this investigation. Detailed information about the material, specimens, strain measurement, and experimental procedures may be found in Wu and Yeh [4] and Wu et al. [24]. We only mention here that initial and

© 2005 by Chapman & Hall/CRC Press

390

Continuum Mechanics and Plasticity 150

Shear stress (MPa)

100

= First P. K. St. = Cauchy St.(th.) = Cauchy St.(ex.) = Second P. K. St.

50

0

–50

–100

–150 350.

450. 550. Axial stress (MPa)

650.

FIGURE 7.28 Subsequent yield surfaces due to tension prestrain determined by various stress measures (From Wu, H.C. et al., J. Appl. Mech., 62, 626, 1995. With permission from ASME).

subsequent yield surfaces were determined for two loading paths. Path (1) in axial loading had an axial prestrain of 20% and path (2) in free-end torsion had a shear prestrain of 20%. After the subsequent yield surface was determined for each loading path, the specimen was removed from the test machine and cut through the cross-section in the middle of the gauge section. By measuring the change of the cross-sectional area, it was found that the reduction of the cross-sectional area was 17% for path (1) and no observable area change was found for path (2). Now the effect of stress measure on the shape, size, and translation of the yield surface is investigated. Figure 7.28 shows the subsequent yield surfaces for path (1). The experimental yield surface (using the 1st P–K stress components) is shown in the middle of the ﬁgure. Also shown in the ﬁgure are the theoretical yield surfaces of the Cauchy stress components determined from (7.161), (7.167), and (7.168) and the 2nd P–K stress components obtained by (7.164). As an independent veriﬁcation, the experimental Cauchy yield surface is also shown in the ﬁgure. The experimental Cauchy stress components were determined based on the measured deformed area. The agreement between the two Cauchy yield surfaces is generally good. However, it may be observed from the ﬁgure that the amount of axial strain affects the size of the Cauchy yield surface. In fact, from (7.167) and (7.168), σ = λ3 T zz and τ = λ3 T zθ and the Cauchy yield surface is an isotropic expansion of

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

391

the 1st P–K yield surface with λ3 being the factor of expansion. For an axial prestrain of 20%, the size of the Cauchy yield surface is about 20% larger than that of the corresponding 1st P–K yield surface. We also note that the translation (the back stress) of the former yield surface is 20% more than that of the latter. In the case of the 2nd P–K stress, we have zθ ∼ = (T zθ /λm ) and zz zz ∼ = (T /λ3 ) from (7.164) for ϕ approximately equal to zero (ϕ is zero during axial prestrain and is very small and negligible during the probing of yield surface). The 2nd P–K yield surface is about 9.5% larger than that of the 1st P–K yield surface in the shear direction but is about 17% smaller in the axial direction. The back stress of the former is 17% less than that of the latter. These results have suggested that the evolution rules for both isotropic and kinematic hardening are stress measure dependent. Figure 7.29 shows the subsequent yield surfaces determined by each stress measure for path (2). Due to no observable change in the cross-sectional area, the Cauchy stress components σ and τ are almost identical to the 1st P–K stress components T zz and T zθ from (7.167) and (7.168). Therefore, the Cauchy and the 1st P–K yield surfaces are indistinguishable in the ﬁgure. However, the components of the 2nd P–K stress are different from those of the Cauchy stress. Using the approximation that all λ’s are equal to 1, (7.164) reduces to zθ ∼ = T zθ − ϕRm T zz and zz ∼ = T zz , that is, the component zθ depends

800

Shear Stress (MPa)

= First P.K. and Cauchy St. (th. and ex.) = Second P.K. St.

500

400

300 –150

0.0 Axial Stress (MPa)

150

FIGURE 7.29 Subsequent yield surfaces due to torsion prestrain determined by various stress measures (From Wu, H.C. et al., J. Appl. Mech., 62, 626, 1995. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

392

Continuum Mechanics and Plasticity

on the twist angle per unit length ϕ. This leads to a rotation of the 2nd P–K surface, with the angle of rotation increasing with the shear strain. It also leads to a further distortion of the 2nd P–K surface in that the yield surface is not symmetric with respect to the shear stress axis. These results complicate the hardening rule associated with the 2nd P–K yield surface. In the aforementioned example, the theoretical results in the case of pretorsion are calculated based on the approximation that all λ’s are equal to 1. Without this approximation, the axial strain exists but is very small. It is less than 0.3% for a prestrain in torsion of 20%. In this case, 1.003 > λ3 > 1 and, from Wu et al. [74] where the circumferential strain was investigated, we obtain 0.9973 < λm < 1. Thus, the effect of this approximation is very small. Also, we emphasize that the rotation and distortion of the 2nd P–K surface is independent of this approximation. EXAMPLE 7.8 Transform the Mises yield criterion in the Cauchy stress space into the stress spaces of the 1st and 2nd P–K stresses.

Solution The Mises yield surface in the Cauchy stress space is (σ − ασ )2 + 3(τ − ατ )2 = k 2

(a)

where ασ and ατ are, respectively, the axial and shear components of the back stress. k is the shear yield stress and is assumed to be constant in this discussion. Using (7.167) and (7.168), (a) is transformed into T

zz

ασ − λ3

2

+3 T

zθ

ατ − λ3

2

=

k λ3

2 (b)

Using (7.164), (b) is further transformed into an equation in the zθ versus zz stress space. In the case of axial prestrain only, ϕ ∼ = 0 and ατ = 0; and using (7.171), the yield function in the zθ versus zz stress space may be written as (zz − (ασ /λ23 ))2 (k/λ23 )

+

(zθ )2 =1 √ (k/ 3λ3 )2

(c)

By comparing equations (a), (b), and (c), we see that the semimajor axes (in the axial stress direction) of the ellipses are k for the Cauchy yield surface, k/λ3 for the 1st P–K surface, and k/λ23 for the 2nd P–K surface. The semiminor axes √ √ √ (in the shear stress direction) are, respectively, k/ 3, k/ 3λ3 , and k/ 3λ3 . The back stress for the three yield surfaces are respectively ασ , ασ /λ3 , and ασ /λ23 . It is seen that the size, shape, and the back stress of the yield surfaces are all inﬂuenced by the deformation of the material element when different stress measures are used.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

393

In the case of torsion only prestrain, ασ = 0. If we use the approximation that all λ’s are one, then the yield surface in the 2nd P–K stress space is governed by the equation (zz )2 + 3[(zθ + ϕRm zz ) − ατ ]2 = k 2

(d)

This equation contains a 6ϕRm zθ zz term, and a rotation in the ellipse will occur. 7.6.6.3 Discussions We have seen from the previous section that the size, shape, and position of the subsequent yield surfaces depend greatly on the stress measure used to deﬁne the yield surface. The different positions of the yield surfaces in the stress space correspond to different degrees of kinematic hardening. We have seen that the hardening rules (isotropic and kinematic hardening) depend greatly on the deﬁnition of stress. The 2nd P–K stress which is often used in the computational mechanics can lead to a yield surface which rotates due to a shear prestrain, while no rotations have been found for this proportional path using the Cauchy stress or the 1st P–K stress. Therefore, the yield surface and the hardening rule should be paired. They vary with the deﬁnition of stress. The yield surface deﬁned by the 2nd P–K stress is independent of imposed rigid-body rotation. In order for the Cauchy yield surface (yield surface deﬁned by the Cauchy stress) to be independent of rigid-body rotation, the yield function has to be a function of stress invariants. The yield surface will be discussed further in Chapter 11 using the true stress in the convected coordinate system. The contravariant components of the true stress do not change with imposed rigid-body rotation.

References 1. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech., 23, 517, 1971. 2. Valanis, K.C., Fundamental consequences of a new intrinsic time measureplasticity as a limit of the endochronic theory, Arch. Mech., 32, 171, 1980. 3. Ohashi, Y. and Tokuda, M., Precise measurement of plastic behavior of mild steel tubular specimens subjected to combined torsion and axial force, J. Mech. Phys. Solids, 21, 214, 1973. 4. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 5. Phillips, A. and Lu, W.Y., An experimental investigation of yield surfaces and loading surfaces of pure aluminum with stress-controlled and strain-controlled paths of loading, J. Eng. Mater. Technol., 106, 349, 1984.

© 2005 by Chapman & Hall/CRC Press

394

Continuum Mechanics and Plasticity

6. Ivey, H.J., Plastic stress–strain relations and yield surfaces for aluminum alloys, J. Mech. Eng. Sci., 3, 15, 1961. 7. Wu, H.C. and Yang, C.C., Investigation of the one-dimensional endochronic constitutive equation for metals by the Rivlin test, J. Eng. Mater. Technol., 106, 264, 1984. 8. Ellis, J.R., Robinson, D.N., and Pugh, C.E., Time dependence in biaxial yield of type 316 stainless steel at room temperature, J. Eng. Mater. Technol., 105, 250, 1983. 9. Taylor, G. I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc. A, 230, 323, 1931. 10. Naghdi, P.M., Essenburg, F., and Koff, W., Experimental study of initial and subsequent yield surface in plasticity, J. Appl. Mech., 201, 1958. 11. McComb, H.G. Jr., Some experiments concerning subsequent yield surface in plasticity, NASA TN D-396, 1960. 12. Mair, W.M. and Pugh, H.L.D., Effect of prestrain on yield surfaces in copper, J. Mech. Eng. Sci., 6, 150, 1964. 13. Bertsch, P.K. and Findley, W.N., An experimental study of subsequent yield surfaces-corners, normality, Bauschinger effect and allied effects, Proc. 4th U.S. Nat. Cong. Appl. Mech., 893, 1962. 14. Phillips, A. and Moon, H., An experimental investigation concerning yield surfaces and loading surfaces, Acta Mech., 27, 91, 1977. 15. Shiratori, E., Ikegami, K., Yoshida, F., Kaneko, K., and Koike, S., The subsequent yield surface after preloading under combined axial load and torsion, Bull. JSME, 19, 877, 1976. 16. Ishikawa, H., Subsequent yield surface probed from its current center, Int. J. Plasticity, 13, 533, 1997. 17. Lode, W., Versuche über den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle, Eisen, Kupfer und Nickel, Z. Phys., 36, 913, 1926. 18. Hu, L.W. and Bratt, J.F., Effect of tensile plastic deformation on yield criterion, J. Appl. Mech., 25, 411, 1958. 19. Szczepinski, W., On the effect of plastic deformation on yield criterion, Arch. Mech., 15, 276, 1963. 20. Szczepinski, W. and Miastkowski, J., An experimental study of the effect of the prestraining history on the yield surfaces of an aluminum alloy, J. Mech. Phys. Solids, 16, 153, 1968. 21. Shiratori, E. and Ikegami, K., Experimental study of the subsequent yield surface by using cross-shaped specimens, J. Mech. Phys. Solids, 16, 373, 1968. 22. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Structures, 8, 463, 1972. 23. Helling, D.E., Miller, A.K., and Stout, M.G., An experimental investigation of the yield loci of 1100-0 aluminum, 70 : 30 brass, and an overaged 2024 aluminum alloy after various prestrains. J. Eng. Mater. Technol., 108, 313, 1986. 24. Wu, H.C., Lu, J.K., and Pan, W.F., Some observations on yield surfaces for 304 stainless steel at large strain, J. Appl. Mech., 62, 626, 1995. 25. Wu, H.C., Effect of loading-path on the evolution of yield surface for anisotropic metals subjected to large pre-strain, Int. J. Plasticity, 19, 1773, 2003. 26. Wu, H.C. and Xu, Z., An axial–torsional extensometer for ﬁnite deformation, J. Eng. Mater. Technol., 112, 330, 1990. 27. Phillips, A., A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity, 2, 315, 1986.

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

395

28. Wu, H.C., Viscoplasticity Under Complex States of Stress, Ph.D. thesis submitted to Yale University, New Haven, CT, 1970. 29. Phillips, A. and Wu, H.C., A theory of viscoplasticity, Int. J. Solids Struct., 9, 15, 1973. 30. Phillips, A., Experimental plasticity. Some thoughts on its present status and possible future trends, in Problems of Plasticity, Sawczuk, A. Ed., Nordhoff International Publishing Leyden, 1974, 193. 31. Krempl, E., Models of viscoplasticity. Some comments on equilibrium (back) stress and drag stress, Acta Mech., 69, 25, 1987. 32. Phillips, A., Liu, K., and Justusson, W.J., An experimental investigation of yield surfaces at elevated temperatures, Acta Mech., 14, 119, 1972. 33. Phillips, A. and Kasper, R., On the foundations of thermoplasticity — an experimental investigation, J. Appl. Mech., 40, 891, 1973. 34. Phillips, A., Tang, J.-L., and Ricciuti, M., Some new observations on yield surfaces, Acta Mech., 20, 23, 1974. 35. Phillips, A. and Kawahara, W.A., The effect of thermal loading on the yield surface of aluminum, An experimental investigation, Acta Mech., 50, 249, 1984. 36. Ohashi, Y., Kawashima, K., and Yokochi, T., Anisotropy due to plastic deformation of initially isotropic mild steel and its analytical formulation, J. Mech. Phys. Solids, 23, 277, 1975. 37. Phillips, A. and Kaechele, L., Combined stress tests in plasticity, J. Appl. Mech., 23, 43, 1956. 38. Khan, A.S. and Wang, X., On non-proportional inﬁnitesimal plastic deformation after ﬁnite plastic prestressing and partial unloading, J. Mech. Phys. Solids, 36, 519, 1988. 39. Mroz, Z., On the description of anisotropic workhardening, J. Mech. Phys. Solids, 15, 163, 1967. 40. Masing, G., Wiss. Veröff. Siemens-Konzern, III Band, 1927. 41. Dafalias, Y.F. and Popov, E.P., A model of nonlinear hardening materials for complex loading, Acta Mech., 21, 173, 1975. 42. Dafalias, Y.F. and Popov, E.P., Plastic internal variables formalism of cyclic plasticity, J. Appl. Mech., 98, 645, 1976. 43. Ilyushin, A.A., On the relation between stresses and small strains in continuum mechanics, Prikl. Mat. Mekh., 18, 641, 1954 (in Russian). 44. Ilyushin, A.A., Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 1963 (in Russian). 45. Lensky, V.S., Analysis of plastic behavior of metals under complex loading, in Proc. 2nd Symposium on Naval Struc. Mech., Lee, E.H. and Symonds, P.S., Eds., Brown University, Pergamon Press, 1960, 259. 46. Ohashi, Y., Tokuda, M., and Tanaka, Y., Precise experimental results on plastic behavior of brass under complex loading, Bull. De L’Acad. Polon. Des Sci., Ser. Sciences Tech., 26, 261, 1978. 47. Ohashi, Y., Kurita, Y., Suzuki, T., and Tokuda, M., Effect of curvature of the strain trajectory on the plastic behavior of brass, J. Mech. Phys. Solids, 29, 69, 1981. 48. Pipkin, A.C. and Rivlin, R.S., Mechanics of rate-independent materials, J. Appl. Math. Phys. (ZAMP), 16, 313, 1965. 49. Zhou, Z.-D., Zhao, S.-X., and Kuang, Z.-B., An integral elasto-plastic constitutive theory, Int. J. Plasticity, 19, 1377, 2003. 50. Ilyushin, A.A., in Problems in the Theory of Plasticity, Izdat. Akad. Nauk. SSSR, Moscow, 1961, 3 (in Russian).

© 2005 by Chapman & Hall/CRC Press

396

Continuum Mechanics and Plasticity

51. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 52. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strainpath, Int. J. Non-Linear Mech., 20, 41, 1985. 53. Wu, H.C., Aboutorabi, M.R., and Chen, P.C.T., Cyclic torsion of a circular cylinder and its residual stress distribution, J. Eng. Mater. Technol., 107, 48, 1985. 54. Wu, H.C. and Yeh, W.C., Some considerations in the endochronic description of anisotropic hardening, Acta Mech., 69, 59, 1987. 55. Wu, H.C. and Ho, C.C., An investigation of transient creep by means of endochronic viscoplasticity and experiment, J. Eng. Mater. Technol., 117, 260, 1995. 56. Green, A.E. and Naghdi, P.M., Ageneral theory of an elastic–plastic continuum, Arch. Rat. Mech. Anal., 18, 251, 1965. 57. Lee, E.H., Elastic–plastic deformations at ﬁnite strains, J. Appl. Mech., 36, 1, 1969. 58. Dafalias, Y.F., A missing link in the macroscopic constitutive formulation of large plastic deformations, in Plasticity Today, Sawczuk, A. and Bianchi, G., Eds., Elsevier Applied Science, London, 1983, 135. 59. Mandel, J., Plasticité classique et viscoplasticité, CISM Courses and Lectures 97, Springer, New York, 1971. 60. Montheillet, F., Cohen, M., and Jonas, J.J., Axial stresses and texture development during the torsion testing of Al, Cu and A-Fe, Acta Metall., 32, 2077, 1984. 61. Stout, M.G. and O’Rourke, J.A., Experimental deformation textures of OFE copper and 70 : 30 brass from wire drawing, compression and torsion, Metall. Trans. 20A, 125, 1989. 62. Toth, L.S., Jonas, J.J., Daniel, D., and Bailey, J.A., Texture development and length changes in copper bars subjected to free-end torsion, Text. Microstruct. 19, 245, 1992. 63. Wang, P.T., Panchanadeeswaran, S., and Wu, H.C., Comparison of ﬂow stress and texture for P0815 cast aluminum deformed in compression and in torsion. Alcoa Technical Center Research Report, Alcoa Center, Pa., U.S.A., 1995. 64. Dafalias, Y.F., Plastic spin: necessity or redundancy?, Int. J. Plasticity, 14, 909, 1998. 65. Kratochvil, J., Finite strain theory of crystalline elastic–inelastic materials, J. Appl. Phys., 42, 1104, 1971. 66. Wang, C.C., A new representation theorem for isotropic functions: an answer to Professor G.F. Smith’s criticism of my paper on representations for isotropic functions, Arch. Rat. Mech. Anal., 36, 166, 1970. 67. Loret, B., On the effects of plastic rotation in the ﬁnite deformation of anisotropic elastoplastic materials, Mech. Mater., 2, 287, 1983. 68. Dafalias, Y.F., The plastic spin, J. Appl. Mech., 52, 865, 1985. 69. Dienes, J.K., On the analysis of rotation and stress rate in deforming bodies, Acta Mech., 32, 217, 1979. 70. Nagtegall, J.C. and de Jong, J.E., Some aspects of non-isotropic workhardening in ﬁnite strain plasticity, in Proc. Workshop on Plasticity of Metals at Finite Strain:

© 2005 by Chapman & Hall/CRC Press

Advances in Plasticity

71. 72. 73. 74. 75. 76.

77. 78. 79. 80.

397

Theory, Experiment and Computation, Lee, E.H. and Mallet, R.L., Eds., Stanford University, 1981, 65. Cotter, B.A. and Rivlin, R.S., Tensors associated with time-dependent stress, Quart. Appl. Math., 18, 177, 1955. Oldroyd, J.G., On the formulation of rheological equations of state, Proc. Roy. Soc., A, 200, 523, 1950. Aifantis, E.C., The physics of plastic deformation, Int. J. Plasticity, 3, 221, 1987. Wu, H.C., Xu, Z., and Wang, P.T., Torsion test of aluminum in the large strain range, Int. J. Plasticity, 13, 873, 1998. Truesdell, C., The simplest rate theory of pure elasticity, Comm. Pure Appl. Math., 8, 123, 1955. Khan, A.S. and Wang, X., An experimental study of large ﬁnite plastic deformation in annealed 1100 aluminum during proportional and nonproportional biaxial compression, Int. J. Plasticity, 6, 485, 1990. Lee, E.H., Mallet, R.L., and Wertheimer, T.B., Stress analysis of anisotropic hardening in ﬁnite-deformation plasticity, J. Appl. Mech., 50, 554, 1983. Wu, H.C., On ﬁnite plastic deformation of anisotropic metallic materials, Int. J. Plasticity, 19, 91, 2003. Wu, H.C., Effect of loading-path on the evolution of yield surface for anisotropic metals subjected to large pre-strain, Int. J. Plasticity, 19, 1773, 2003. Wu, H.C. and Xu, Z., An experimental investigation of the axial effect during torsion, in Advances in Constitutive Laws for Engineering Materials, Fan, J. and Murakami, S., Eds., Int. Academic Publishers, Pergamon Press, Beijing, 1989, 232.

Problems (1) Write a report about additional experimental evidence showing the normality of the plastic strain increment to the subsequent yield surface. (2) Write a report about Ilyushin’s isotropy postulate. (3) Referring to Figure 7.18 in a stress-controlled loading problem, how do surfaces fA , fB , and fC move when the stress point follows path PQ? (4) Derive (7.97) from (7.95). (5) In simple shear problem using Cotter–Rivlin stress rate, show that the solution is given by (7.107) for hypoelastic materials. (6) In simple shear problem using Truesdell’s stress rate, show that the solution is given by (7.110) for hypoelastic materials. (7) In the problem of rectangular metal block discussed in Example 7.3, if µ = 26 GPa and λ = 33 GPa, plot the σx versus Dx dt and σz versus Dx dt curves. In addition, plot Dy as a function of Dx and discuss the effect of h on the results. (8) Use the Jaumann rate to investigate and plot the loading–unloading curve of simple shearing. The material is rigid-plastic with linear kinematic hardening.

© 2005 by Chapman & Hall/CRC Press

398

Continuum Mechanics and Plasticity During loading, the simple shear deformation is governed by x1 = X1 + 2ωtX2 ,

x2 = X2 ,

x3 = X3

and its displacement ﬁeld is u1 = 2ωtX2 ,

u2 = u3 = 0,

ω = const

The unloading starts at t* and the displacement ﬁeld during unloading is u1 = [2ωt ∗ −2ω(t − t∗)]x2 = 2ω(2t ∗ −t)x2 ,

u2 = u3 = 0,

for t > t ∗ .

(9) Show that (7.101) may be derived from (7.100). (10) Solve Problem (8) using the Dafalias rate. (11) Solve Problem (8) using Lee’s rate. (12) Find the physical components of deformation gradient F in the spherical coordinate system. (13) In an uniaxial stress test, the following data have been recorded for the axial stress–strain curve: (plastic strain, stress (MPa))={(0, 100), (0.005, 289.59), (0.01, 336.82), (0.02, 369.03), (0.04, 397.35), (0.06, 420.78), (0.1, 458.86), (0.14, 489.12), (0.2, 526.71)}. The stress has been calculated based on the undeformed cross-sectional area. Plot the equivalent stress versus equivalent plastic strain curves using the Cauchy stress, the 1st P–K stress and the 2nd P–K stress as stress measure, respectively. (14) In a torsion test of thin-walled tubular specimen, the following data have been recorded for the shear stress–strain curve: ( plastic shear strain, shear stress (MPa))={(0, 100), (0.005, 273.36), (0.01, 309.48), (0.02, 334.87), (0.04, 362.20), (0.06, 387.10), (0.1, 428.59), (0.14, 469.60), (0.2, 521.34)}. The stress has been calculated based on the undeformed cross-sectional area. Plot the equivalent stress versus equivalent plastic strain curves using the Cauchy stress, the 1st P–K stress and the 2nd P–K stress as stress measure, respectively. Compare these curves with those obtained in Problem (13).

© 2005 by Chapman & Hall/CRC Press

8 Internal Variable Theory of Thermo-Mechanical Behaviors and Endochronic Theory of Plasticity

8.1

Introduction

There are several approaches to irreversible thermodynamics. One of them, the internal variable theory, is widely used in recent literature of mechanics of solids. In this chapter, the concept and equations of the internal variable theory of irreversible thermodynamics, which are used to describe the thermo-mechanical behavior of materials are ﬁrst discussed. Based on this thermodynamic foundation, it is shown how a theory of plasticity, known as the endochronic theory, can be developed. Applications of the endochronic theory to metals, geotechnical materials, and damage mechanics are then discussed in this chapter and Chapter 9. The theory of thermodynamics that is presented owes much to the work of Valanis [1–4]. A summary of Valanis’ works on the internal variable theory of thermodynamics is nicely presented in [5], although it does not contain recent works on the gradient theory. The gradient theory is outside scope of this book, but readers are referred to [4] for further reading. The endochronic theory of plasticity was developed by Valanis [6,7] and this author had the privilege of learning the theory directly from Professor Valanis and has been heavily involved in the further development and veriﬁcation of the theory. Other researchers have also made signiﬁcant contributions to the theory.

8.2 8.2.1

Concepts and Terminologies of Thermodynamics The First Law of Thermodynamics

Irreversible thermodynamics is also known as the nonequilibrium thermodynamics. It is needed because we are dealing with an irreversible system, which is a material region R. A reversible system exists only in an ideal gas or an ideal elastic material. It is assumed that the system possesses an internal 399

© 2005 by Chapman & Hall/CRC Press

400

Continuum Mechanics and Plasticity

energy E with density ε (read also Section 4.3.3). Readers are referred to Callen [8] for measurability of internal energy. The mechanical variables are stress, deformation, and mass. In addition, temperature is a variable. Amechanical process is a process during which energy (in the absence of heat supply, e.g., heat sources) is transmitted to the system through an adiabatic boundary by motion of the boundary and/or application of long-range forces. The adiabatic boundary is a boundary through which no heat can ﬂow. This type of energy is called work, denoted by W . A thermal process is a process during which energy ﬂows through the boundary of the system and/or is supplied to its interior while its boundary remains stationary and there are no long range (gravitational, say) forces acting. This type of energy is called heat, denoted by Q. Conduction is a process during which energy is supplied to the system by heat ﬂow through its boundary. A boundary and/or a process which is not adiabatic will be called diathermal. Conduction is a diathermal process. The ﬁrst law of thermodynamics is a statement of the conservation of energy discussed in Section 4.3.3. In the local form, which applies to an inﬁnitesimal neighborhood of a material region, the energy balance equation is from (4.34) ρ ε˙ = σki vi,k − hi,i + ρ q˙

(8.1)

where ρ is the current mass density; hi is the heat ﬂux vector, in which the direction of the vector is the direction of the heat ﬂow; q is the internal energy supply per unit mass by radiation or “other sources” such as electric conductors; and the dot denotes the material differentiation. We note that |hi | is the amount of energy ﬂow per unit area normal to the direction of heat ﬂow per unit time. Referring to the undeformed conﬁguration, the energy balance equation is from (4.68) ε˙ =

1 ∂hR 1 1 ˙ RS E˙ RS − + q˙ = RS E˙ RS + Q ρ0 ρ0 ∂XR ρ0

˙ =− with Q

1 ∂hR + q˙ ρ0 ∂XR (8.2)

˙ is the rate of heat supply per unit volume (conduction and radiation). where Q

8.2.2

State Variables, State Functions, and the Second Law of Thermodynamics

The change of internal energy may be accomplished through (1) a purely thermal process (radiation, heat conduction, etc.), which changes the temperature of the system, or (2) an adiabatic process, that is, work, which changes the position of the boundary and causes the system to deform. Thus, strain and temperature are measures of the internal energy of the system. They are called state variables, since they serve to deﬁne the state of the system. Internal

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

401

energy is a state function, which is a function of state variables. The thermodynamic state of the system is represented by the state functions. One of the main tasks of thermodynamics is to establish those quantities that are state functions and those that are not and to establish useful relationships between state functions. In a reversible system, the internal energy and stress are state functions written as ε = ε(ERS , T)

and

RS = RS (EPQ , T)

(8.3)

where ERS is the strain and T the temperature. The fundamental issue is that the increment of heat supply dQ is not an exact differential. The meaning of this statement is not obvious without further clariﬁcations and deﬁnitions. A reversible system is said to undergo a reversible process if its thermodynamic state is being changed under adiabatic conditions. It is an irreversible process when the process is diathermal. In this case, dQ is not an exact differential, where dQ = 0 following a closed contour in the (ERS , T) space. From (8.2), we have

dε =

1 RS dERS + ρ0

dQ

(8.4)

The integral on the left-hand side is zero because ε is a state function given by (8.3). The ﬁrst integral on the right-hand side represents the amount of work done on the system, which in general is not zero when the path of integration involves thermal processes. The statement may be better understood by examining the Carnot cycle, which is a reversible cycle for ideal gas carried out with the piston–cylinder arrangement. The Carnot cycle goes through two reversible isothermal processes connected by two reversible adiabatic processes and the work done is not zero. Thus, from (8.4) dQ = 0

(8.5)

Hence, dQ is not an exact differential and we cannot write Q = Q(ERS , T). However, in the case of an ideal gas, dQ/T is an exact differential in the sense that dQ/T = 0. Therefore, deriving dS = dQ/T, we ﬁnd that dS is an exact differential. Thus, in the case of a gas dQ = T dS(ERS , T), where S = S(ERS , T), which is a state function known as entropy. An important contribution by Valanis [2] is the proof of the existence of entropy in irreversible systems, establishing the entropy as a state function. We now consider the reversible system and leave the irreversible system for later discussion. In the case of the reversible system, the energy equation (8.2) is written as dε −

1 RS dERS = dQ = θ(ERS , T) dη(ERS , T) ρ0

© 2005 by Chapman & Hall/CRC Press

(8.6)

402

Continuum Mechanics and Plasticity

where θ is the integrating factor; η is the speciﬁc entropy, and (8.6) is integrable so that η is a state function, that is, η = η(ERS , T). The equation dη = gQ/θ is also known as the second law of thermodynamics. The factor θ(ERS , T) has the signiﬁcance of empirical temperature. We note that entropy is dimensionless, and temperature has the dimensions of energy [8]. The units of temperature depend on the nature of the thermometric substance used. Temperature measured by a mercury thermometer is not exactly the same as that given by an electrical resistance thermometer except at their common points. Degree Kelvin is the absolute temperature. Using (8.3), (8.6) is ∂ε ∂ε 1 dERS + dT − RS dERS = θ ∂ERS ∂T ρ0

∂η ∂η dERS + dT ∂ERS ∂T

(8.7)

Since ERS and T can be independently varied and dERS and dT are arbitrary, the following are obtained 1 ∂ε ∂η RS = −θ ρ0 ∂ERS T ∂ERS T

and

∂ε ∂η =θ ∂T ∂T

(8.8)

Since θ = θ (ERS , T), we can express the state functions as ε = ε(θ , ERS ) and η = η(θ , ERS ). Using the chain rule of differentiation, we have ∂ε ∂ε = ∂T ∂θ ERS ∂ε ∂ERS T ∂η ∂ERS T

∂θ ∂η ∂η ∂θ , = ∂T ERS ∂T ∂θ ERS ∂T ERS ∂θ ∂ε ∂ε = + ∂θ ERS ∂ERS T ∂ERS θ ∂θ ∂η ∂η = + ∂θ ERS ∂ERS T ∂ERS θ

(8.9)

By substituting (8.9) into (8.8), we obtain ∂ε ∂η 1 RS = − θ ∂ERS θ ∂ERS θ ρ0

and

∂ε ∂η =θ ∂θ ∂θ

(8.10)

This equation has the same form as (8.8). It shows that the form of the equation is independent of the temperature scale used, and the state functions can be expressed as ε = ε(ERS , θ ) and RS = RS (EPQ , θ). We now introduce a new state function, deﬁned by (ERS , θ) = ε − θη, which is known as the Helmholtz free energy. Differentiating , we have ∂ ∂ε ∂η = −θ ∂ERS θ ∂ERS θ ∂ERS θ

© 2005 by Chapman & Hall/CRC Press

and

∂ ∂ε ∂η = −θ − η. ∂θ ∂θ ∂θ

Internal Variable Theory and Endochronic Theory

403

We then substitute these expressions into (8.10) to obtain 1 ∂ RS = ρ0 ∂ERS

and

η=−

∂ ∂θ

(8.11)

These are the constitutive equations for reversible systems.

8.3 8.3.1

Thermodynamics of Internal State Variables Irreversible Systems

In some systems, the state functions are not uniquely determined by the state variables ERS and T of the system. For instance, in materials undergoing plastic deformation, the current state of stress will depend on the whole history of the deformation. In the case of uniaxial loading–unloading at constant temperature, the stress, which is a state function, is not uniquely determined by the strain E11 , as shown in Figure 8.1. Both points A and B have the same strain, but the states of the internal structure of the material are different at the two points. It is therefore necessary to introduce other macroscopic parameters, additional to strain and temperature, which are representative of the internal structure of the material. Another example that shows the inadequacy of the state of strain in predicting the state of stress is given in Figure 8.2. We represent the unknown material to be tested at constant temperature by a black box. Within the black box there are the spring and dashpot elements with elastic moduli E1 and E2 for the springs. If we do not know the internal structure of the black box and test it macroscopically, the state of stress σ cannot be described uniquely in terms of the state of strain of the black box. Other parameters (internal variables) will have to be used in order to determine the stress. However, if we Π11

A

B E11

FIGURE 8.1 Stress not uniquely determined by strain.

© 2005 by Chapman & Hall/CRC Press

404

Continuum Mechanics and Plasticity Black Box E1

E2

Dashpot

FIGURE 8.2 Test of black box.

open the black box and know the internal structure and constitution of the black box, that is, we know the properties and arrangement of the springs and the dashpot, then we know that the overall strain of the black box is the same as the strain of spring 1, and, if we also know the strain of the dashpot as a function of time, we are able to describe the stress uniquely. The strain of the dashpot is the internal variable needed to uniquely describe the stress. For this example, the stress is a function of the overall strain and the strain of the dashpot. In the materials modeling, n parameters may be needed to uniquely deﬁne the stress state. These parameters are called internal (state) variables and are denoted by qr , where r = 1, . . . , n. Internal state variables are called internal coordinates by some authors. They can be scalars, but, generally, they are tensors. It is assumed that sufﬁcient additional state variables (not all observable) can always be found to describe the thermodynamic state of an irreversible system. As previously mentioned, the internal state variables are the macroscopic representations of microscopic effects that have physical meanings. They may represent observed effects due to slips at the crystallographic level or represent dislocations, etc. Owing to the difference in scale, these effects may not be directly observable at the macroscopic scale and are represented by the internal variables. In the mechanics literature, some investigators have been able to identify the physical meanings of their internal variables at the microscopic level. In that case, they are able to use the evolution rules for those physical quantities obtained from experiments at the microscopic level. Mathematically speaking, the internal variables are state variables and the state functions are deﬁned in terms of the state variables. As long as the evolution equations are provided for the state variables, the problem can be solved without assigning physical meanings to the internal variables. For an irreversible system, the state functions are functions of strain, temperature, and n numbers of internal variables, and they are represented by ε = ε(ERS , θ , qrRS ), r = 1, . . . , n

© 2005 by Chapman & Hall/CRC Press

η = η(ERS , θ , qrRS ),

RS = RS (EPQ , θ , qrRS ), (8.12)

Internal Variable Theory and Endochronic Theory

405

Valanis [2] proved the existence of an entropy function η and that the Pfafﬁan form (8.6) of the ﬁrst law of thermodynamics is integrable even for irreversible systems, and thus the entropy is a state function. In an earlier effort, Valanis showed that the constitutive equations for irreversible systems are 1 ∂ε ∂η RS = −θ ρ0 ∂ERS θ,qr ∂ERS θ,qr PQ

and

PQ

∂ε ∂η =θ ∂θ EPQ ,qr ∂θ EPQ ,qr PQ

PQ

(8.13) Valanis [2] assumed that the system behaves reversibly when qrRS are constants and dqrRS = 0 for all r. The derivation from (8.6) to (8.10) can then be used to establish (8.13) for irreversible systems. By using the Helmholtz free energy = ε − ηθ, where = ψ(ERS , θ , qrRS ), (8.13) is further written as 1 ∂ RS = ρ0 ∂ERS

and

η=−

∂ ∂θ

(8.14)

These are powerful results and were independently obtained by Valanis [1] and Coleman and Gurtin [9].

8.3.2

The Clausius–Duhem Inequality

By putting ε = + ηθ into the ﬁrst law of thermodynamics (8.6), we have d + η dθ + θ dη −

1 RS dERS = dQ ρ0

(8.15)

or ∂ ∂ ∂ 1 dERS + dθ + r dqrRS + η dθ + θ dη − RS dERS = dQ ∂ERS ∂θ ∂qRS ρ0 (8.16) Using (8.14), (8.16) is reduced to θ dη +

∂ dqr = dQ ∂qrRS RS

(8.17)

The second term on the left-hand side of (8.17) is absent in a reversible system. In the rate form, (8.17) may be rewritten as ∂ θ η˙ + r ∂qRS E

PQ ,θ

© 2005 by Chapman & Hall/CRC Press

˙ q˙ rRS = θ η˙ + E

PQ,θ

˙ =Q

(8.18)

406

Continuum Mechanics and Plasticity

˙ EPQ ,θ = (∂/∂qr )|EPQ ,θ q˙ r is the rate of change of the Helmholtz The term | RS RS free energy under constant strain and temperature. We now invoke the Kelvin postulate which states that the free energy cannot increase if the strain and the temperature are kept constant, [5]. The postulate is thus written in the mathematical form as ˙ EPQ ,θ ≤ 0 |

(8.19)

˙ EPQ ,θ θ γ˙ ≡ −|

(8.20)

If we deﬁne

then, from (8.19) and (8.20), we obtain γ˙ ≥ 0

(8.21)

where γ˙ is known as the entropy production. Substituting (8.20) into (8.18), we have η˙ =

˙ Q + γ˙ θ

(8.22)

˙ Q θ

(8.23)

which results in η˙ ≥

This inequality is known as the Clausius–Duhem inequality, and the equality holds only for reversible systems. Using (8.22), (8.18) may be written as ˙ + θ γ˙ ) + (Q

∂ r ˙ q˙ = Q ∂qrRS RS

(8.24)

which reduces to θ γ˙ = −

∂ r q˙ ≥ 0 ∂qrRS RS

(8.25)

This is an alternate form for the Clausius–Duhem inequality.

8.3.3

The Helmholtz Formulation of Thermo-Mechanical Behavior

Most of the discussions in the previous section belong to the Helmholtz formulation. We summarize the equations of this formulation here for later reference.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

407

First law of thermodynamics: ε˙ =

1 1 ∂hR RS E˙ RS − + q˙ ρ0 ρ0 ∂XR

(8.26)

Clausius–Duhem (rate of dissipation) inequality: −

∂ r q˙ ≥ 0 ∂qrRS RS

(8.27)

Heat conduction equation: hR = hR (EPQ , θ , θ,P , qrPQ )

(8.28)

where θ,R is the temperature gradient. Equation (8.28) is a generalized form of Fourier’s law of heat conduction, which states that the heat ﬂux vector is proportional to the temperature gradient θ,R . The state functions are = (ERS , θ , qrRS ), η = η(ERS , θ , qrRS ),

ε = ε(ERS , θ , qrRS ) RS = RS (EPQ , θ , qrPQ )

(8.29)

The relations between state functions are RS = ρ0

∂ , ∂ERS

η=−

∂ ∂θ

(8.30)

These relations apply to all materials irrespective of their constitution. The internal state variables qrRS represent the constitutive nature of the material. These internal variables distinguish one material from the other. In an elastic material, qrRS = 0; whereas in a viscoelastic material, qrRS = 0, and the change of qrRS is governed by a set of evolution equations for qrRS . From (8.27), the rate of change q˙ rRS should be related to ∂/∂qrRS so that the inequality is not violated. The simplest relation between the two quantities is expressed in terms of a functional relationship so that q˙ rRS

=

r fRS

∂ ∂qrPQ

r = fRS (EPQ , θ , qrPQ )

where r = 1, . . . , n

(8.31)

The last expression in (8.31) is obtained due to = (EPQ , θ , qrPQ ). The evolution equations for qrRS of a material undergoing plastic deformation will be discussed later in conjunction with the endochronic theory of plasticity.

© 2005 by Chapman & Hall/CRC Press

408

Continuum Mechanics and Plasticity

r , the expressions for Knowing , h,R , and fRS RS and η can be obtained r are subject to the constraints from (8.30). The forms of hR and fRS

−

∂ r q˙ ≥ 0 ∂qrRS RS

and

hR θ,R ≤ 0

(8.32)

The second inequality of (8.32) describes the nature of heat conduction. Heat ﬂows from high to low temperature. In the Helmholtz formulation, there are 22 + n equations. They are listed below with the number of equations shown at the end of the equations: Conservation of mass Equation of motion Conservation of energy Strain–displacement equations ∂(EPQ , θ , qrPQ ) RS = ρ0 ∂ERS ∂(EPQ , θ , qrPQ ) η=− ∂θ ε = ε(EPQ , θ , qrPQ ) or = (EPQ , θ , qrPQ ) hR = hR (EPQ , θ , θ,P , qrPQ ) r (E , θ , qr ) q˙ rRS = fRS PQ PQ

1 3 1 6 6

(8.33)

1 1 3 n

The 22 + n unknowns are ρ(1), RS (6), η(1), ε(1), hR (3), the displacements ui (3), ERS (6), θ (1), and qrRS (n), with the number of unknowns shown inside the parenthesis. Thus, the solution for the set of equations can be determined.

8.3.4

The Gibbs Formulation of Thermo-Mechanical Behavior

The Gibbs formulation is complementary to the Helmholtz formulation. In the Helmholtz formulation, strain is the independent variable and stress is the dependent variable; in the Gibbs formulation, stress is the independent variable and strain is the dependent variable. Thus, the state functions are functions of RS , θ , and qrRS . The energy equation is from (8.26) ε˙ =

1 ∂hR 1 RS E˙ RS − + q˙ ρ0 ρ0 ∂XR

(8.34)

For an irreversible system at constant qrRS , following Valanis [2], we may write ε˙ |qrPQ −

© 2005 by Chapman & Hall/CRC Press

1 RS E˙ RS = θ η| ˙ qrPQ ρ0

(8.35)

Internal Variable Theory and Endochronic Theory

409

Let = ε − ηθ , we have ˙ qr = ε˙ |qr − ηθ˙ − η| ˙ qrPQ θ | PQ PQ

(8.36)

Substituting (8.36) into (8.35), we obtain ˙ qr − | PQ

1 RS E˙ RS + ηθ˙ = 0 ρ0

(8.37)

The Gibbs free energy is now deﬁned as =−

1 RS ERS ρ0

(8.38)

By differentiation, we then have ˙ qr = | ˙ qr + | PQ PQ

1 1 ˙ RS ERS RS E˙ RS |qrPQ + ρ0 ρ0

(8.39)

Substituting (8.39) into (8.37), we obtain ∂ 1 ∂ ˙ RS + ˙ RS ERS + ηθ˙ = 0 θ˙ + ∂RS θ,qr ∂θ PQ ,qr ρ0 PQ

(8.40)

PQ

Since the stress and the temperature can be arbitrarily varied, it is concluded that ∂ ∂ (8.41) ERS = −ρ0 and η = − ∂RS θ,qr ∂θ PQ ,qr PQ

PQ

These are the constitutive equations in the Gibbs formulation. In the following functions, we note the differences in the independent variables: E = E(, θ, qr ), = (, θ, qr ), but = (E, θ , qr ). Differentiating (8.38), we have ˙ = ˙ −

1 1 ˙ RS ERS − RS E˙ RS ρ0 ρ0

(8.42)

or ∂ ∂ ∂ ˙ RS + θ˙ + r q˙ rRS ∂RS ∂θ ∂qRS =

∂ ˙ ∂ 1 1 ∂ ˙ RS ERS − RS E˙ RS ERS + θ˙ + r q˙ rRS − ∂ERS ∂θ ∂qRS ρ0 ρ0

© 2005 by Chapman & Hall/CRC Press

(8.43)

410

Continuum Mechanics and Plasticity

Using (8.14) and (8.41), (8.43) reduces to ∂ ∂ r q˙ RS = r q˙ rRS r ∂qRS ∂qRS

(8.44)

The Clausius–Duhem inequality (8.32) becomes ∂ r ∂ q˙ = r q˙ rRS ≤ 0 ∂qrRS RS ∂qRS

(8.45)

The evolution equations for qrRS are r (PQ , θ , qrPQ ) q˙ rRS = gRS

(8.46)

r must satisfy the constraint of Clausius–Duhem Note that the functions gRS r is related to f r by the inequality. In addition, from (8.31) and (8.46), gRS RS equation r r = fRS [EPQ (TU , θ , qsTU ), θ , qsTU ] gRS

with r, s = 1, . . . , n

(8.47)

r can be nonlinear. However, linear functions work extremely The functions gRS well for applications to be discussed in connection with the endochronic theory. In the case of linear functions, the evolution equations are

∂ + brRSPQ q˙ rPQ = 0 ∂qrRS

(r not summed)

(8.48)

where brRSPQ is a positive deﬁnite fourth-rank tensor. Knowing , an explicit form of constitutive equations can be obtained.

8.4 8.4.1

The Endochronic Theory of Plasticity The Concepts of the Endochronic Theory

Valanis developed the endochronic theory of plasticity in two major papers [6,7]. The Greek word endochronic means intrinsic (or internal) time. The deformation history is represented by a monotonically increasing time-like parameter ζ known as the endochronic (or intrinsic) time. The endochronic time accounts for the intrinsic material properties and is deﬁned as dζ 2 = PRSPQ dERS dEPQ

© 2005 by Chapman & Hall/CRC Press

(8.49)

Internal Variable Theory and Endochronic Theory

411

where PRSPQ is a fourth-rank tensor, which could depend on ERS . This concept of intrinsic time is different from that of Ilyushin [10] and Pipkin and Rivlin [11], using the arc length of the strain path as a parameter. In that case, dζ 2 = dERS dERS

(8.50)

We note that (8.50) is a special case of (8.49). Another original idea of Valanis’ is to develop a theory that describes the stress–strain curve without a yield surface. The stress–strain curves of metals such as aluminum, brass, and high-strength steel do not show an apparent yield point. As we have discussed in Section 6.2, several deﬁnitions of yield surfaces are available and there are factors affecting the experimental determination of yield surfaces. Valanis tried to avoid the use of yield surface and showed in [6] that, using the thermodynamics of the internal variable and the concept of intrinsic time, it was indeed possible to develop a theory which not only does not have a yield point but can also successfully describe metal behaviors such as the Baushinger effect in unloading behavior, hardening due to shear prestrain, cyclic stress–strain loops, and cyclic hardening. At the time when [6] was published, the ﬂow theory of plasticity was not yet successful in theoretically describing these complex behaviors of metals. This theory of Valanis [6] is simple in form and will be referred to as the simple endochronic theory. This theory has many advantages because of its simplicity in calculation. Take the cyclic loading as an example, the ﬂow theory of plasticity would need to determine whether the current state is in the plastic state and, if so, apply the ﬂow rule, which is incremental. An intense numerical integration is needed. The equations of the endochronic theory, on the other hand, may be integrated to obtain a closed form solution without having to determine the yield point. However, there are drawbacks of the simple endochronic theory. The unloading curve has a slope slightly larger than the initial slope of the stress–strain curve. If, in a plastic state, a small amount of stress unloading occurs and is immediately followed by a reloading back to the original stress level, then a stress–strain loop does not form. If this unloading–reloading cycle continues, then cyclic creep or ratcheting would occur without reaching a steady state, that is, the strain would continue to increase as the stress cycling continues, but not in agreement with experimental ﬁndings. Another drawback is related to the rate of entropy production. In a plastic state, increments in loading and unloading will result in the same rate of entropy production, which is not acceptable. Despite the drawbacks, the simple endochronic theory continues to be used by some investigators because of its simplicity and because the concept of yield surface is not needed. It provides a good approximation to metals when only loading is of interest, or under certain loading histories such as cyclic loading. An improved endochronic theory, or simply the “endochronic theory” in the remainder of this chapter, was proposed by Valanis [7] to remove the aforementioned drawbacks. The improved theory uses plastic strain to deﬁne the

© 2005 by Chapman & Hall/CRC Press

412

Continuum Mechanics and Plasticity

intrinsic time, while the simple endochronic theory uses the total strain. Valanis [7] showed that a limiting case of this new formulation leads to the deﬁnition of yield surface. In fact, the ﬂow theory of plasticity can be derived from the endochronic theory, including the ﬂow rule and the strainhardening rules. However, the forms of the ﬂow rule and strain-hardening rules are derived; whereas these forms and rules are separately assumed in the traditional ﬂow theory of plasticity. This author has been heavily involved in the development and veriﬁcation of the endochronic theory. Specially designed experiments have been conducted by the author and his coworkers which are then used to verify the theory. These investigations will be discussed in later sections of this chapter and in Chapter 9. 8.4.2

The Simple Endochronic Theory of Plasticity

The simple endochronic theory has been derived for small isothermal deformation in [6], using the Helmholtz formulation discussed in Section 8.3.3. In the small deformation, the stress is σ and the strain is ε. Equation (8.30) reduces to σ=

∂ , ∂ε

η=−

∂ , ∂θ

−

∂ · q˙ r ≥ 0 ∂qr

(r not summed)

(8.51)

From the last expression of (8.51), we see that q˙ r cannot be independent of −∂/∂qr . Otherwise, an arbitrary choice of q˙ r may violate the inequality. Therefore, q˙ r and −∂/∂qr must be related. The relation can be in the form of a function or of a functional, or something else. For the sake of simplicity, a function is assumed in the ensuing discussion. Furthermore, a linear form is assumed such that ∂ + brijkm q˙ rkm = 0 ∂qrij

(r not summed)

(8.52)

where brijkm is a symmetric positive deﬁnite tensor. Note that this linear form has been proven to be adequate in most applications. Other forms may be considered if called for. However, we like the linear form because of its mathematical simplicity. Substituting (8.52) into the last expression of (8.51), we obtain brijkm q˙ rij q˙ rkm ≥ 0

(r not summed)

(8.53)

The intrinsic time is from (8.49) dζ 2 = Pijkm dεij dεkm

© 2005 by Chapman & Hall/CRC Press

(8.54)

Internal Variable Theory and Endochronic Theory

413

In the endochronic theory, all developments are with respect to the increment of intrinsic time. The evolution equation for the internal variables can then be expressed with respect to the intrinsic time as dqr ∂ + brijkm (ζ ) km = 0 r ∂qij dζ

(r not summed)

(8.55)

where brijkm (ζ ) is a function of intrinsic time ζ and brijkm = (br0 )ijkm f (ζ ); (8.55) may then be written as dqr ∂ + (br0 )ijkm f (ζ ) km = 0 r ∂qij dζ

(r not summed)

(8.56)

or dqrkm ∂ r + (b ) =0 ijkm 0 ∂qrij dz

(r not summed)

(8.57)

where (br0 )ijkm is a fourth-rank constant tensor; the intrinsic time has been scaled by a factor f and z is the intrinsic timescale. The relation is dζ f (ζ )

dz =

(8.58)

The scaling factor f (ζ ) will be identiﬁed later as the isotropic hardening function. The case of f = 1 corresponds to no isotropic hardening. Generally, (8.58) may be integrated from the initial intrinsic time ζ0 to the current intrinsic time ζ as z=

ζ

ζ0

dζ f (ζ )

(8.59)

As a ﬁrst approximation, we use the linear form f (ζ ) = 1 + βζ

(8.60)

and, in this case, (8.59) becomes z=

1 ln(1 + βζ ) β

with initial values ζ0 = z0 = 0; β is a constant.

© 2005 by Chapman & Hall/CRC Press

(8.61)

414

Continuum Mechanics and Plasticity

In summary, the endochronic equations of the Helmholtz formulation for small isothermal deformation are = (ε, qr ), dz =

σ=

dζ , f (ζ )

∂ , ∂ε

r ∂ r dq + b = 0, · 0 ∂qr dz

(8.62)

dζ 2 = dε · P · dε

where a boldfaced letter with an underscore, such as P, denotes a fourth-rank tensor. To obtain an explicit constitutive equation, the free energy is expressed in a quadratic form as = 21 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr

(8.63)

where A , Br , Cr are fourth-rank constant tensors. Note that linear terms in ε are absent to accommodate the requirement that the reference state is unstressed. In addition, linear terms in qr are absent if the reversal of the sign of strain history leaves the form of the stress response invariant. Substituting (8.63) into (8.62), we obtain σ=A·ε+

Br · q r

Br · ε + Cr · qr + br0 ·

and

r

dqr =0 dz

(8.64)

If A, Br , Cr and br0 are isotropic functions and, since σ, ε, and qr are symmetric tensors, the isotropic expressions for these tensors are from (1.129) Aijkm = A1 δij δkm + A2 δik δjm ,

Brijkm = Br1 δij δkm + Br2 δik δjm ,

r Cijkm = C1r δij δkm + C2r δik δjm ,

(br0 )ijkm = br1 δij δkm + br2 δik δjm

(8.65)

Substituting (8.65) into (8.64) and separating the resulting equations into the hydrostatic and deviatoric parts, we ﬁnd σkk = (3A1 + A2 )εkk + (3Br1 + Br2 )qrkk σij

= A2 eij +

r

(8.66)

Br2 pijr

r

Br0 εkk + C0r qrkk + br0 Br2 eij + C2r pijr + br2

dqrkk =0 dz

dpijr dz

(r not summed)

(8.67)

=0

where the deviatoric parts are eij = εij − 13 δij εkk ,

© 2005 by Chapman & Hall/CRC Press

σij = σij − 13 δij σkk ,

pijr = qrij − 13 δij qrkk

(8.68)

Internal Variable Theory and Endochronic Theory

415

and A0 = 13 (3A1 + A2 ),

Br0 = 13 (3Br1 + Br2 ),

C0r = 13 (3C1r + C2r ),

br0 = 13 (3br1 + br2 )

(8.69)

Equations in (8.67) are constant coefﬁcient linear ordinary differential equations and the solutions are Br z Cr exp − r0 (z − z ) εkk (z ) dz with qrkk (0) = 0 qrkk = − r0 b0 z0 b0 (8.70) Br2 z C2r r

r exp − r (z − z ) eij (z ) dz with pij (0) = 0 pij = − r b2 z0 b2 Combining (8.66) and (8.70) yields σ =

1 σkk = 3

z z0

K(z − z )

dεkk dz dz

σij = 2

and

z

z0

µ(z − z )

deij dz dz (8.71)

where the kernel functions are given by K(z) = A0 −

(Br )2

2µ(z) = A2 −

0 C0r

r

(Br )2 2

r

C2r

H(z) +

(Br )2 0 C0r

r

H(z) +

e−λr z

(Br )2 2

r

C2r

with λr =

C0r br0 (8.72)

e−ρr z

Cr with ρr = r2 b2

where H(z) is the Heaviside step function. These kernel functions are also known as the heredity functions. If 2µ(z) is plotted against

z, the curve has a value of A2 at z = 0 and relaxes gradually to [A2 − r ((Br2 )2 /C2r )] as z increases and becomes large. Similarly, K(z) has an initial value of A0 and relaxes to

(A0 − r ((Br0 )2 /C0r )). The functions µ(z) and K(z) are sums of positive decaying exponential terms, where one or more of the exponents may be zero. This describes the effect of fading memory. In the event that the hydrostatic response is elastic as most metals are, Br0 = C0r = 0 and qrkk is constant. The ﬁrst equation of (8.72) reduces to K(z) = A0 H(z)

(8.73)

and the hydrostatic stress–strain curve is from (8.71) σ = 13 σkk = A0 εkk

© 2005 by Chapman & Hall/CRC Press

(8.74)

416

Continuum Mechanics and Plasticity

Valanis and Wu [12] investigated the representation of heredity functions and showed that the theory was able to describe observed behavior of metals under conditions of cyclic deformation. In addition, Wu and his coworkers [13–16] applied the theory to investigate the problem of viscoplastic wave propagation in thin rods and thin-walled tubes. By differentiation, the deviatoric part of the constitutive equation in (8.71) can be written in a differential form. In the simple case of µ(z) = µ0 e−αz , where µ0 and α are constants, we have σ = 2µ0

z

e−α(z−z )

0

de dz dz

(8.75)

and dσ = (−α)2µ0 dz

z

e−α(z−z )

0

de de dz + 2µ0

dz dz

(8.76)

or dσ de + ασ = 2µ0 dz dz

(8.77)

This is the constitutive equation in the differential form. From (8.77), we see that the plastic strain increment is dep = de −

dσ α = dzσ 2µ0 2µ0

(8.78)

This is in the form of the Prandtl–Reuss relation, when the elastic strain is considered. On the other hand, the function µ(z) may contain more terms. For example, µ(z) = µ0 + µ1 e−αz , where µ0 , µ1 , and α are constants. We then obtain dep =

α µ0 σ dz − αe dz 2µ¯ µ¯

with µ¯ = µ0 + µ1

(8.79)

Equation (8.79) is not in the form of the Prandtl–Reuss relation. EXAMPLE 8.1

Determine the endochronic constitutive equation for uniaxial

tension. Solution In uniaxial tension, (8.71) reduces to σ =

© 2005 by Chapman & Hall/CRC Press

z 0

E(z − z )

dε dz dz

(a)

Internal Variable Theory and Endochronic Theory

417

The stress is σ , the strain is ε, and E(z) is the heredity function. We assume that the specimen is initially in an annealed state so that z0 = 0. We consider the simplest case possible, when E(z) has only one exponential term, that is, E(z) = E0 e−αz

(b)

where E0 and α are constants. The intrinsic time increment is from (8.54) dζ = ±k dε

(c)

in which k is assumed to be a constant for simplicity. The positive and negative sign in (c) are for loading and unloading. We use the linear form for intrinsic timescale given by (8.60), which is integrated to yield (8.61). We then obtain from (8.61) the expression 1 + βζ = eβz , which leads to dζ = eβz dz

(d)

where β is a constant. Substituting (b) into (a) and using (c) and (d), we obtain σ = E0

z

e−α(z−z )

0

dε dζ dz = E0 dζ dz

z

e−α(z−z )

0

1

(eβz )dz k

eβz

E0 E0 (1 + βζ ) [1 − e−(α+β)z ] = [1 − (1 + βζ )−(1+α/β) ] k(α + β) kβ(1 + α/β) α E0 1 with n = 1 + = (1 + βζ ) 1 − kβn (1 + βζ )n β

=

(e)

In loading starting from zero load and zero strain, (c) can be integrated to yield ζ = kε

(f)

Using (f), (e) becomes σ =

E0 1 (1 + β1 ε) 1 − β1 n (1 + β1 ε)n

with β1 = kβ

(g)

This is the endochronic stress–strain relation with three parameters E0 , β1 , and n. This equation is able to describe the stress–strain curve for most metallic materials. The three parameters may be determined by a method described in Example 8.2. A method by use of the optimization technique is given by Jao et al. [17].

© 2005 by Chapman & Hall/CRC Press

418

Continuum Mechanics and Plasticity Et

0

E0 FIGURE 8.3 A stress–strain curve.

EXAMPLE 8.2

Determine the three parameters of the endochronic stress–

strain relation σ =

E0 1 (1 + β1 ε) 1 − β1 n (1 + β1 ε)n

(a)

Solution A hypothetical experimental stress–strain curve is shown in Figure 8.3, and we like to determine E0 , β1 , and n so that (a) describes this experimental curve. We ﬁrst determine E0 , Et , and σ 0 from the experimental curve. E0 is the slope at ε = 0; Et is the tangent modulus at large ε; and σ 0 is the intercept of the asymptote of the stress–strain curve with the stress axis. We note that E0 = (dσ /dε)|ε→0 , and this is about the same as Young’s modulus for materials that has a very straight initial curve. E0 should be slightly larger than the conventional value for Young’s modulus, if the material starts to bend right from the beginning of the stress–strain curve. The asymptote at large ε is found from (a) as σ =

E0 (1 + β1 ε) β1 n

(b)

with slope dσ E0 Et = = dε ε→large n

(c)

Therefore, n=

© 2005 by Chapman & Hall/CRC Press

E0 Et

(d)

Internal Variable Theory and Endochronic Theory

419

The intercept of the asymptote with the stress axis is found by setting ε = 0 in (b). Thus, σ0 =

E0 β1 n

(e)

β1 =

E0 nσ 0

(f)

From (e), we obtain

Therefore, knowing E0 , Et , and σ 0 , we ﬁnd n from (d) and β1 from (f). EXAMPLE 8.3

If the free energy is positive deﬁnite, that is, = 12 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr > 0

(a)

and if r Cijkm = C1r δij δkm + C2r δik δjm

Aijkm = A1 δij δkm + A2 δik δjm ,

(b)

show that A1 + 13 A2 > 0,

A2 > 0

and

C1r + 13 C2r > 0,

C2r > 0

(c)

Solution The free energy is positive deﬁnite, > 0, for any ε and qr subjected to the thermodynamic constraints discussed in Section 8.3.3. In a special case, > 0 for ε = 0 and arbitrary nonzero qr , so that = 12 qr · Cr · qr > 0

(d)

Therefore, Cr must be positive deﬁnite. Another special case is when qr = 0 subjected to nonzero arbitrary ε. Then, = 12 ε · A · ε > 0

(e)

that is, A must be positive deﬁnite. Using (b) and (e), we have = 12 (A1 εii εkk + A2 εik εik )

© 2005 by Chapman & Hall/CRC Press

(f)

420

Continuum Mechanics and Plasticity

which may be written in the matrix form as T ε11 ε22 ε33 ε12 1 T ε13 = [ε] [A][ε] = 2 ε 21 ε21 ε31 ε32 A1 A1 0 0 0 0 0 0 ε11 A1 + A2 ε22 A1 A + A A 0 0 0 0 0 0 1 2 1 A1 A1 A1 + A 2 0 0 0 0 0 0 ε33 0 0 0 2A2 0 0 0 0 0 ε12 0 0 0 0 2A2 0 0 0 0 ε13 × 0 0 0 0 0 0 0 2A2 0 ε21 0 0 0 0 0 0 2A2 0 0 ε21 0 0 0 0 0 0 0 2A2 0 ε31 ε32 0 0 0 0 0 0 0 0 2A2 (g)

Since is positive deﬁnite, [A] is a positive deﬁnite matrix, that is, the determinant of every principal minor should be nonnegative. Therefore, (a) A1 + A2 > 0

(h)

A1 + A2 (b) A1

= A2 (2A1 + A2 ) > 0 A1 + A 2

A1 + A2 (c) A1 A1

A1 A1 + A 2 A1

A1 A1 = A22 (3A1 + A2 ) > 0 A1 + A 2

A1 A1 + A 2 A1 0

A1 A1 A1 + A 2 0

A1 + A2 A1 (d) A1 0

A1

(i)

0 0 = (2A2 )A2 (3A1 + A2 ) > 0 2 0 2A2

(j)

(k)

From (h) to (k), it is concluded that A2 > 0,

A1 + A2 > 0,

© 2005 by Chapman & Hall/CRC Press

2A1 + A2 > 0,

3A1 + A2 > 0

(m)

Internal Variable Theory and Endochronic Theory

421

Plotting the above inequalities in the A2 versus A1 space, it is found that the solution is bounded by A2 > 0

3A1 + A2 > 0

and

(n)

Using a similar procedure, the following inequalities can be established C1r + 13 C2r > 0

and

C2r > 0

(o)

An alternate proof is obtained by considering simple loading conditions. We rewrite (f) as A2 1 1 (p) A1 + (εkk )2 + A2 eik eik = 2 3 2 In the case of hydrostatic strain, the strain components are ε11 = ε22 = ε33 = ε and eij = 0, (p) reduces to =

1 A2 A1 + (3ε)2 > 0 2 3

or

A1 +

A2 >0 3

(q)

In the case of shear with ε12 = 0 and other εij = 0, we have from (p) = A2 (e12 )2 > 0

or

A2 > 0

(r)

The physical meanings are not clear if the same procedure is applied to = 12 qr · Cr · qr > 0. 8.4.3

The Improved Endochronic Theory of Plasticity

Valanis [7] used a strain-like tensor Qij to deﬁne the intrinsic time as dζ 2 = dQij dQij

where Qij = εij − Kijkm σkm

(8.80)

This deﬁnition of intrinsic time is a generalization of (8.54). In onedimensional straining, (8.80) reduces to dσ dζ = |Q| = dε − k1 E 0

with 0 ≤ k1 ≤ 1

(8.81)

When k1 = 0, dζ = |dε|, which is the simple endochronic theory; but when k1 = 1, Q has the meaning of plastic strain. This new deﬁnition of intrinsic time removes the drawbacks mentioned for the simple endochronic theory, and, in addition, the case of k1 = 1 leads to the existence of yield surface. We shall demonstrate the latter assertion in the discussions to follow.

© 2005 by Chapman & Hall/CRC Press

422

Continuum Mechanics and Plasticity

We ﬁrst show that the deviatoric constitutive equation of (8.71) σ = 2

z

z0

µ(z − z )

de dz = 2µ0 dz

z z0

ξ(z − z )

de dz dz

(8.82)

may be written in the following form σ = 2µ0

z 0

ρ(z − z )

dQ dz dz

(8.83)

where Q = e − k1

σ , 2µ0

µ(z) = µ0 ξ(z),

ξ(0) = 1

(8.84)

The relation between ξ(z) and ρ(z) may be found by the method of Laplace transformation. From (8.82), we have σ¯ = 2µ0 ξ¯ p¯e

with e(0) = 0

(8.85)

where f¯(p) is the transform of the function f (z) and p is the parameter of Laplace transformation. We note that L(df (z)/dz) = pf¯(p) − f (0). On the other hand, (8.83) is transformed into ¯ ¯ Q σ¯ = 2µ0 ρp

with Q(0) = 0

(8.86)

Using the Laplace transform of (8.84), (8.86) is further written as

σ¯ = 2µ0 ρp ¯ e¯ − k1

σ¯ 2µ0

(8.87)

Substituting (8.85) into (8.87), the resulting equation is ¯ ξ¯ = ξ¯ ρ¯ − k1 ρp

(8.88)

¯ ξ¯ − ξ(0)) − k1 ρξ(0) ¯ = ξ¯ ρ¯ − k1 ρ(p

(8.89)

which may be written as

An inverse transform of (8.89) gives us (1 − k1 )ρ(z) − k1

© 2005 by Chapman & Hall/CRC Press

z 0

ρ(z − z )

dξ dz = ξ(z) dz

with ξ(0) = 1

(8.90)

Internal Variable Theory and Endochronic Theory

423

It can be shown that, for k1 = 1, the solution of (8.90) is ρ(z) = ρ0 δ(z) + ρ1 (z)

(8.91)

where ρ1 (z) =

n−1

Rr e−βr z ,

ξ(z) =

r=1

n

ξr e−αr z ,

r=1

n

ξr = 1

(8.92)

r=1

and δ(z) is the Dirac delta function; Rr , ξr , βr , αr , and ρ0 are constants. Using (8.91) and (8.92), (8.83) becomes σ = 2µ0 ρ0

dQ(z) + 2µ0 dz

z 0

ρ1 (z − z )

dQ(z ) dz dz

(8.93)

Equation (8.93) is the constitutive equation of the endochronic theory. This equation may be used directly to calculate the stress–strain response curves. On the other hand, based on this equation, the ﬂow rule, the yield surface, and its hardening rules can be derived, thereby establishing a connection between the present theory and the ﬂow theory of plasticity. By doing so, the physical meanings of some functions and parameters of this theory become clear. The differences between this theory and the ﬂow theory are that the forms of the ﬂow rule, yield surface, and hardening rule are related in this theory and they evolve with respect to the intrinsic time, while they are quite open to differently proposed forms in the classical ﬂow theory. In the following subsection, we derive the ﬂow rule, the yield surface, and the hardening rule. EXAMPLE 8.4

In the simple case of ξ(z) = ξ1 e−α1 z + ξ2 e−α2 z

(a)

determine the expression for ρ(z). Solution The Laplace transform of (a) is ξ¯ (p) =

ξ1 ξ2 + p + α1 p + α2

(b)

Substituting (b) into (8.88), we have ρ¯ =

ξ¯ (p) p+λ = 2 ¯ (1 − k1 )p + (α1 + α2 − k1 λ)p + α1 α2 1 − k1 pξ (p)

© 2005 by Chapman & Hall/CRC Press

(c)

424

Continuum Mechanics and Plasticity

where λ = ξ1 α2 + ξ2 α1 . In the case of k1 → 1, (c) becomes ρ¯ ≈

p+λ p+λ = (1 − k1 )(p + β1 )(p + β2 ) (1 − k1 )p2 + (α1 + α2 − λ)p + α1 α2

(d)

where β1 =

λ¯ , 1 − k1

β2 =

α1 α2 , λ¯

λ¯ = α1 ξ1 + α2 ξ2

(e)

Equation (d) may be further written as ρ¯ =

1 1 − k1

((λ − β1 )/(β2 − β2 )) ((λ − β2 )/(β1 − β2 )) + p + β1 p + β2

(f)

which may then be inverse transformed into 1 ρ(z) = 1 − k1

λ − β1 −β1 z λ − β2 −β2 z e + e β2 − β 1 β1 − β 2

(g)

Using (e), we ﬁnd that λ − β1 ≈1 β2 − β 1

and

λ − β2 1 λλ¯ − α1 α2 ≈ 1 − k 1 β1 − β 2 λ¯ 2

(h)

Therefore, (g) becomes 1 α1 α2 λ¯ λλ¯ − α1 α2 ρ(z) = exp − exp − z + z 1 − k1 1 − k1 λ¯ 2 λ¯

(i)

When k1 → 1, (i) reduces to ρ(z) = ρ0 δ(z) +

λλ¯ − α1 α2 λ¯ 2

α1 α2 exp − z = ρ0 δ(z) + ρ1 (z) λ¯

(j)

Thus, ρ1 (z) =

© 2005 by Chapman & Hall/CRC Press

λλ¯ − α1 α2 λ¯ 2

α1 α2 exp − z λ¯

(k)

Internal Variable Theory and Endochronic Theory 8.4.4

425

Derivation of the Flow Theory of Plasticity from Endochronic Theory

In the case of k1 = 1, the deviatoric part of the endochronic constitutive equation is from (8.93) σ = 2µ0 ρ0

dQ(z) + 2µ0 dz

z 0

ρ1 (z − z )

dQ(z ) dz dz

(8.93)

with the intrinsic time deﬁned from (8.80) by p

dζ 2 = dQij dQij

where dQij = dεij = deij −

dσij 2µ0

(8.94)

If we let α = 2µ0

z 0

ρ1 (z − z )

dQ(z ) dz dz

and

σy = 2µ0 ρ0

(8.95)

then, (8.93) can be written as dQ f (z) + α dζ

(8.96)

dζ (σ − α) σy f (z)

(8.97)

σ = σy which may be further written as dQ =

This equation may be considered as the ﬂow rule using the concept of the ﬂow theory of plasticity. By substituting (8.97) into (8.94), we obtain 2

dζ = dQ · dQ =

dζ

σy f (z)

2 (σ − α) · (σ − α)

(8.98)

or [(σ − α) · (σ − α) − (σy f (z))2 ]dζ 2 = 0

(8.99)

Therefore, we obtain from (8.99) either (σ − α) · (σ − α) = (σy f (z))2

with dζ 2 = 0

(8.100)

or dζ 2 = 0

© 2005 by Chapman & Hall/CRC Press

(8.101)

426

Continuum Mechanics and Plasticity

Equation (8.100) is the yield criterion with combined isotropic–kinematic hardening. α represents the back stress and f (z) represents the isotropic hardening. We will call f (z) the isotropic-hardening function. The yield criterion applies when p

p

dζ 2 = dQij dQij = dεij dεij p

p

p

p

p

p

= (dε11 )2 + (dε22 )2 + (dε33 )2 + 2(dε12 )2 + 2(dε23 )2 + 2(dε31 )2 = 0 (8.102) p

Since all terms in (8.102) are positive, dεij = 0 when dζ 2 = 0. dζ 2 = 0 only when all components of the plastic strain increments are zero. The case of dζ 2 = 0 is given by (8.101) and further written as 2

dζ =

p p dεij dεij

= deij −

dσij

dσij

deij − 2µ0 2µ0 dσ 2 dσ 2 dσ 2 = de11 − 11 + de22 − 22 + de33 − 33 2µ0 2µ0 2µ0 2 2

2 dσ12 dσ23 dσ31 + 2 de12 − + 2 de23 − + 2 de31 − =0 2µ0 2µ0 2µ0 (8.103)

Since all terms in (8.103) are positive, dζ 2 = 0 only when all terms are zero, that is, deij −

dσij 2µ0

=0

or

dσij = 2µ0 deij

and

σij = 2µ0 eij

(8.104)

When all components of the plastic strain increments are zero, the material behavior is described by (8.104), which is the elastic constitutive equation. We have thus shown that the ﬂow theory of plasticity may be derived from the endochronic theory when k1 = 1. The yield function is given by (8.100); the ﬂow rule is given by (8.97); the back stress is given by (8.95); and the isotropic hardening is given by the function f (z). We see from (8.97) that the normality condition between the plastic strain increment and the yield surface (8.100) is satisﬁed. The evolution of back stress may be written in a differential form by differentiating (8.95). If, for simplicity, only one exponential term is used in ρ1 (z), that is, ρ1 (z) = ρˆ e−αz , where ρˆ and α are constants, then α = 2µ0 ρˆ

© 2005 by Chapman & Hall/CRC Press

0

z

e−α(z−z )

dεp (z ) dz dz

(8.105)

Internal Variable Theory and Endochronic Theory

427

and dα dεp = 2µ0 ρˆ − αα dz dz

(8.106)

This is a nonlinear evolution equation for α and was used by Wu and Yang [18] and Wu et al. [19] as mentioned in Section 6.5.3. This equation is also known as the Armstrong–Frederick evolution equation. Another special case of (8.95) is when ρ1 (z) = ρˆ = constant. In this case, (8.95) becomes α = 2µ0 ρε ˆ p

or

dα = c dεp

with c = 2µ0 ρˆ

(8.107)

which is the linear kinematic hardening of Prager [20] and Ziegler [21]. In the general case, when ρ1 (z) is given by (8.92), the evolution equation for α is dεp dα 2G0 Rr β r αr = − dz dz n−1

n−1

r=1

8.4.5

with α =

r=1

n−1

αr

(8.108)

r=1

Applications of the Endochronic Theory to Metals

The endochronic theory is applied to describe several aspects of metallic deformation. They include loading–unloading, cyclic loading, loading with multi-axial strain paths, and the viscoplastic effect. Additional applications will be discussed in Chapter 9. 8.4.5.1

The loading–unloading stress–strain curves

In the case of uniaxial stress, the endochronic constitutive equation is σ = E0

z 0

ρ(z − z )

dε p dz dz

(8.109)

We investigate three functional forms of the isotropic-hardening function f (z). They are: Form (a): f (z) = eβz , and

Form (b): f (z) = C − (C − 1)e−βc z ,

Form (c): f (z) = e−βs z

(8.110)

The equation dζ /dz = f (z) is plotted in the ζ versus z space in Figure 8.4(a) for the three forms. The slope of the asymptote for form (a) is ∞, that for form (b) is C, and for form (c) is 0. The curve of form (c) approaches a value of 1/βs when z is large. The straight line at 45◦ angle is the case of f (z) = 1, which represents the nonhardening behavior. This line separates the ζ –z space into hardening zone and softening zone. When form (b) is used, the value of C dictates the material behavior. The case of C > 1 corresponds to strain

© 2005 by Chapman & Hall/CRC Press

428

Continuum Mechanics and Plasticity

(a) 10

(b)

C>1

10

8

f = C–(C–1)e–z, final slope = C

6 4

2

6 0C z∗ and the integral in (8.109) is divided into two integrals σ = E0

z∗ 0

ρ(z − z )

dε p dz + E0 dz

z z∗

ρ(z − z )

dε p dz dz

(8.116)

Using (8.111) as the kernel function, the ﬁrst integral of (8.116) consists of three terms. They are E0

0

E1

z∗

z∗

0

δ(z − z )[C − (C − 1)e−βc z ]dz = 0,

= E1 e E2

z∗

0

e−α(z−z ) [C − (C − 1)e−βc z ]dz −αz

C −αz∗ C − 1 −(βc −α)z∗ − 1) + − 1) , (e (e α βc − α

(8.117)

dζ dz = E2 ζ ∗ dz

The second integral also has three terms, given by

z

z∗ z

E0 E1

z∗

δ(z − z )(−1)[C − (C − 1)e−βc z ]dz = −σy [C − (C − 1)e−βc z ],

= −E1 E2

z 0

e−α(z−z ) (−1)[C − (C − 1)e−βc z ]dz

(−1)

C C − 1 −βc z ∗ ∗ ∗ (e − e−α(z−z )−βc z ) (1 − e−α(z−z ) ) + α α − βc

(8.118)

dζ dz = −E2 (ζ − ζ ∗ ) dz

Using (8.117) and (8.118), (8.116) is reduced to σ = − σy [C − (C − 1)e −

−βc z

]+

σ0 ∗ − σy C[2 e−α(z−z ) − e−αz − 1] C

σ0 C−1 ∗ ∗ [2 e−α(z−z )−βc z − e−αz − e−βc z ] + E2 (2ζ ∗ − ζ ) − σy α C α − βc (8.119)

During the unloading stage, the following relation holds dζ = −dεp

© 2005 by Chapman & Hall/CRC Press

∗

with initial condition ζ ∗ = εp

(8.120)

Internal Variable Theory and Endochronic Theory

431

Integration of (8.120) results in ε p = 2ζ ∗ − ζ

(8.121)

The loading–unloading curves have been calculated and compared with experimental results for 304 stainless steel by Wu and Yip [22]. 8.4.5.2

A strain-controlled cyclic loading

Since most experiments have been conducted by controlling the total strain amplitude ε, a small amount of approximation is involved in this theoretical representation by considering a constant plastic strain amplitude cycling. Figure 8.6(a) shows a schematic drawing for strain cycles plotted against time t and the notation used to denote intrinsic time z at each half cycle. Figure 8.6(b) shows the corresponding cyclic stress–strain curve. The loading in the previous subsection can be viewed as the ﬁrst 41 cycle which is valid (a) Strain Control

z3*

z*

z7*

z5*

t

z2*

z4*

∆

z6*

(b) Cyclic Hardening Hysteresis Loops z(2N)* z5* z3* z* Stable

1 D

D

z2* z4* z(2N)* FIGURE 8.6 (a) Strain cycles against time, (b) cyclic hardening hysteresis loops (From Wu, H.C. and Yip, M.C., J. Eng. Mater. Technol., 103, 212, 1981. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

432

Continuum Mechanics and Plasticity

for 0 < z < z∗ and the unloading in the previous subsection can be viewed as the ﬁrst unloading of the cyclic loading valid for z∗ < z < z∗∗ . We continue to derive the equations for the ﬁrst reloading and the subsequent loading. ∗ Using the same procedure, the ﬁrst reloading is valid for z∗∗ < z < z3 and the equation has been found to be σ0 ∗∗ σ = σy [C − (C − 1)e ]+ − σy C[−2 e−α(z−z ) C C−1 σ0 −α(z−z∗ ) −α + 2e − e z + 1] − − σy α C α − βc −βc z

× [−2e−α(z−z

∗∗ )−β z∗∗ c

+ 2e−α(z−z

+ E2 (ζ + 2ζ ∗ − 2ζ ∗∗ )

∗ )−β z∗ c

− e−αz + e−βc z ]

with ε p = 2ζ ∗ − 2ζ ∗∗ + ζ

(8.122)

This procedure may be continued. A general expression of the response function for the constant total strain amplitude cyclic loading test may be found to be σ = (−1)2N σy [C − (C − 1)e−βc z ] σ0 ∗ ∗∗ − σy C{1 − e−αz + 2[e−α(z−z ) − 1] − 2[e−α(z−z ) − 1] + C 2N ∗

+ · · · − [(−1)2N 2][e−α(z−z ) − 1]} σ0 α(C − 1) −βc z ∗ ∗ − {e − e−αz + 2[e−α(z−z )−βc z − e−βc z ] − σy C α − βc − · · · − (−1)2N 2[e−α(z−z + E2 ε p

for z > z2N

2N ∗ )−β z2N ∗ c

− e−βc z ]}

∗

(8.123)

where ∗

εp = ζ + 2(ζ ∗ − ζ ) − 2(ζ ∗∗ − ζ ) + · · · − (−1)2N · 2(ζ 2N − ζ )

(8.124) ∗

and N = 12 , 1, 1 12 , 2, . . . . If the above equation is examined at z = z2N ∗ and z = z2N + , a ∗drop or jump in stress of magnitude 2σy f (z) = 2N 2σy [C − (C − 1)e−βc z ] results, which corresponds to the elastic response upon reversal of loading direction. The magnitude of the jump in stress is determined by the isotropic expansion of the yield surface. For a sufﬁciently large z, the hysteresis loop becomes steady. In this case the jump or drop in stress becomes a constant value of 2Cσy .

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

433

MPa ksi Cyclic Stress–strain Curve

12½ Stable

150 20

3½

100

2½ 10

50

1½ N=½

–1.0

–0.6

–0.2

0.2

0.6

1.0

%

–50 –10 –100 –150

Theory

–20 Experiment from [23] N = ½ and 1 N = 1½ and 2 N = 2½ and 3 N = 3½ and 4 N = 8½ and 9 (Stable)

FIGURE 8.7 Theory and experimental data (From Wu, H.C. and Yip, M.C., J. Eng. Mater. Technol., 103, 212, 1981. With permission from ASME).

We now use (8.123) to predict the cyclic stress–strain loops experimentally obtained by Lamba and Sidebottom [23]. These authors obtained cyclic stress– strain curves of oxygen-free high-conductivity copper covering curves from the ﬁrst cycle to the stable loop. The hardening effect was extremely rapid in the ﬁrst few cycles of the test. After further reversals, hardening ceased and a steady stress range was achieved. Figure 8.7 illustrates the experimental data and the theoretical prediction from (8.123). The material parameters used in the calculation are: σ 0 = 25 ksi (1.73 × 102 MPa), σy = 2 ksi (13.78 MPa), E2 = 0, C = 8.75, βc = 40, α = 3000, and ε = 1.75%. Finally, we mention that the same theory was applied by Wu et al. [24] to investigate the problem of cyclic full-reversed torsional loading of a solid bar with circular cross-section. Numerical techniques were employed to obtain the solution. The parameters of the constitutive model were determined from the test data of thin-walled specimens. These parameters were then used without alteration to compute stress distributions within the solid specimen.

© 2005 by Chapman & Hall/CRC Press

434

Continuum Mechanics and Plasticity

Special attention was given to the residual stress distribution. Reasonable results were obtained. The relation of torque versus strain at the outermost ﬁber of the solid specimen provided an ultimate check of the theory as applied to this case.

8.4.5.3 Loading with multiaxial strain path From (8.93), the constitutive equation for metals is

σ =

dε σy

p (z)

dz

+ 2µ2

z

e−α(z−z )

0

dε p (z ) dz + 2µ1 ε p dz

(8.125)

where σy is the deviatoric yield stress; µ1 and µ2 are constants. The volumetric behavior is elastic, given by (8.74). Only one exponential term in the kernel function is used for simplicity. We applied (8.125) to describe two strain-controlled combined axial–torsion tests (paths 01A and 02B) shown in Figure 8.8. Form (b) of (8.110) is the isotropic-hardening function used in this derivation. The state of stress and its deviator and the plastic strain are 2σ 3

[σ ] = τ 0

σ τ 0 [σ ] = τ 0 0 , 0 0 0

τ σ − 3 0

p ηp 0 ε p εp η − p 0 [ε ] = 2 εp 0 0 − 2 (8.126)

0

0 , σ − 3

where ηp is the tensorial shear strain. The intrinsic time is obtained from dζ 2 = dε p · K · dε p

B

1

0 FIGURE 8.8 Two strain paths of combined axial–torsion.

© 2005 by Chapman & Hall/CRC Press

(8.127)

A

2

Internal Variable Theory and Endochronic Theory

435

as dζ = [k12 (dε p )2 + k22 (dηp )2 ]1/2

(8.128)

where k1 and k2 are constants. We follow the work of Wu and Yang [25] in the following discussion with permission from Elsevier. (A) Path 01A The specimen is ﬁrst strained in pure torsion from 0 to 1 (Figure 8.8) and then strained in tension from 1 to A while keeping the total shear strain constant. p The plastic shear strain at 1 is denoted by η∗ , the corresponding shear stress ∗ ∗ by τ , and the intrinsic time by z . There are two stages in this path. The ﬁrst stage is straining from 0 to 1 and the second stage from 1 to A. We have a pure torsion in the ﬁrst stage and the equations are from (8.125) τ=

dη σy

p

+ 2µ2

dz

z

e−α(z−z )

0

dηp dz + 2µ1 ηp dz

and

σ =0

(8.129)

Since during this stage, dζ = k2 dηp , (8.129) may be integrated. In the second stage, (8.125) gives σ = 1.5

dε σy

p

dz

+ 2µ2

z z∗

e

−α(z−z ) dε

p

dz

dz + 2µ1 ε

p

(8.130)

and τ = σy

dηp + 2µ2 X e−αz + 2µ2 dz

z z∗

e−α(z−z )

dηp dz + 2µ1 ηp dz

(8.131)

where X=

0

z∗

eαz

dηp 1 dz =

dz k2

C αz∗ C − 1 (α−β)z∗ − 1] [e − 1] − [e α α−β

(8.132)

Equation (8.131) may be reduced to a closed-form expression for τ in terms of z, which is accomplished by use of the following procedure. We note that η remains constant during this stage and we have dηp = −

dτ 2µ0

(8.133)

in which µ0 is the shear modulus. (8.133) is then integrated to yield p

ηp = η∗ −

© 2005 by Chapman & Hall/CRC Press

1 (τ − τ ∗ ) 2µ0

(8.134)

436

Continuum Mechanics and Plasticity

Letting z −z∗ = t and z −z∗ = t and making use of (8.133) and (8.134), (8.131) may be written as −σy dτ µ2 t −α(t−t ) dτ −α(t+z∗ ) τ= + 2µ2 e X− e dt 2µ0 dt µ0 0 dt 1 p + 2µ1 η∗ − (t − t∗ ) 2µ0

(8.135)

Laplace transform of (8.135) gives τ¯ =

¯ Q R¯ ∗

=

p

p{(p + α)σy τ ∗ + 4µ0 µ2 e−αz X + 2µ2 τ ∗ } + 4µ0 µ1 (η∗ + (τ ∗ /2µ0 ))(p + α) p{σy p2 + [ασy + 2(µ0 + µ1 + µ2 )]p + 2(µ0 + µ1 )α} (8.136)

which, by partial fraction, can be reduced to τ¯ =

2 µ 0 µ1 p µ0 + µ 1

p

η∗ +

τ∗ 2µ0

+

A B +

p−α p − β

(8.137)

where τ¯ is the Laplace transform of τ (z) and A, B, α , β are constants. Con¯ ¯ )/R¯ (α ), B = Q(β ¯ )/R¯ (β ), = 0; A = Q(α stants α and β are the zeros of R(p)

¯ ¯ ¯ and R¯ (p) = dR/dp. The functions Q(p) and R(p) are deﬁned in (8.136). Finally, (8.137) may be inverted to yield τ=

2µ0 µ1 µ0 + µ 1

p

η∗ +

τ∗ 2µ0

∗

+ A eα (z−z ) + B eβ (z−z

∗)

(8.138)

which is the expression relating τ to z. The equation for axial stress (8.130) may be written in a form convenient z

for numerical computation. Let S = z∗ e−α(z−z ) (dε p /dz )dz ; then by differentiating this integral with respect to z, we obtain dS dεp = − αS dz dz

(8.139)

in which, when dε p /dz is known, S may be computed step by step. Thus, σ may be found from dε p σ = 1.5 σy + 2µ2 S + 3µ1 ε p dz

© 2005 by Chapman & Hall/CRC Press

(8.140)

Internal Variable Theory and Endochronic Theory

437

The quantity dε p /dz is computed from the equation below which is found from (8.128) and (8.133)

dε p dz

2

1

=

k12

dζ dz

2

−

k2 2G0

2

dτ dz

2 (8.141)

The quantity dζ /dz is given by form (b) of (8.110) and dτ/dz is found by differentiation of (8.138). Therefore, by assuming a value for z, τ , and dτ/dz may be computed from (8.138), and dεp /dz may be found from (8.141). Using the latter value, S can be found step by step from (8.139) and σ can be obtained from (8.140). Furthermore, knowing the value of dε p /dz and using (8.133), ε p and ηp can be computed. (B) Path 02B The specimen is ﬁrst strained in pure tension from 0 to 2 (Figure 8.8) and then strained in torsion from 2 to B while keeping the total axial strain constant. p The plastic tensile strain at 2 is denoted by ε∗ , the corresponding tensile stress ∗ ∗ by σ , and the intrinsic time by zˆ . There are two stages in this path. The ﬁrst stage is straining in pure tension from 0 to 2, and the second stage from 2 to B. The equations for stage 1 are

dε σy

σ = 1.5

p

dz

+ 2µ2

z

e

−α(z−z ) dε

p

dz

0

dz + 2µ1 ε

p

τ =0

and

(8.142) and the equations for stage 2 are z p dε p

dε e−α(z−z ) dz + 2µ1 ε p + 2µ2 Y e−αz + 2µ2 σ = 1.5 σy dz dz zˆ ∗

(8.143)

and τ=

dη σy

p

dz

+ 2µ2

z zˆ ∗

e−α(z−z )

dηp dz + 2µ1 ηp dz

(8.144)

where Y=

zˆ ∗

e 0

αz dε

p

1 dz = dz k1

C αˆz∗ C − 1 (α−β)ˆz∗ [e − 1] − [e − 1] α α−β

(8.145)

Following a similar procedure as in Path 01A, we ﬁnd E0 Et σ = E0 + E t

© 2005 by Chapman & Hall/CRC Press

p ε∗

σ∗ + E0

ˆ eαˆ (z−ˆz∗ ) + Bˆ eβˆ (z−ˆz∗ ) +A

(8.146)

438

Continuum Mechanics and Plasticity

dε p = − Sˆ =

z

zˆ ∗

dσ E0

e−α(z−z )

(8.147)

dηp dz dz

(8.148)

dηp dSˆ = − α Sˆ dz dz dηp + 2µ2 Sˆ + 2µ1 ηp τ = σy dz

(8.149) (8.150)

and

dηp dz

2

=

1 k22

dζ dz

2

−

k1 E0

2

dσ dz

2 (8.151)

ˆ Bˆ are constants; E0 is Young’s modulus and Et = 3µ1 . in which αˆ , βˆ , A, Assuming a value for z, σ , and dσ/dz may be computed from (8.146), and dηp /dz may be found from (8.151). Using the latter value, Sˆ can be found step by step from (8.149) and τ can be obtained from (8.150). Furthermore, knowing the value of dηp /dz and using (8.147), ε p and ηp can be computed. For the purpose of assessing the validity of the derived equations, the theoretical results are compared with the experimental data obtained by Ohashi et al. [26] for thin-walled tubular brass (60% Cu, 40% Zn) specimens. The constants of the theory have been determined in [25] to be σy = 95.02 MPa, β = 4.3996, C = 4.5799, µ0 = 12.74 GPa, µ2 = 6.37 GPa, µ1 = 49.0 MPa, k1 = 1, and α = 500. The material response for Path 01A is shown in Figure 8.9 after torsion prestrain of ηp = 4.33 × 10−3 , 8.66 × 10−3 , 17.32 × 10−3 , and 25.98 × 10−3 . It is seen that the theory agrees well qualitatively with the experiment. There are quantitative discrepancies between the theory and experiment at the knee portion of the axial stress curve, however. In addition, the theory predicted a faster relaxation of shear stress than the experimental data indicated. Ohashi and his coworkers [27,28] have described the same experimental data using the simple endochronic theory with very good agreement. Ohashi et al. made the kernel function a tensor quantity. Thus, different stress components are associated with different components of the kernel function and the parameters are different for each component of the kernel function. In addition, the intrinsic time was made a function of the arc length as well as the radius of curvature of the strain path. More parameters have been introduced into the theory by this generalization. Using the method of solution of Wu and Yang [25], the endochronic constitutive equation (8.125) was applied by Wu et al. [29] to investigate the stress response to two cyclic, nonproportional strain paths in the axial–torsion strain space. The ﬁrst path involved a cyclic axial straining and unstraining following a shear prestrain, and the second path was cyclic in shear after a

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory 30

280

Axial

27 240

18 15 12 9

Stress ( or ) MPa

Stress ( or ) Kgf/mm2

24 21

200

Theory data by Ohashi et al. (1978)

160

p = 4.33 × 10–3

120

p = 8.66 × 10–3 p = 17.32 × 10–3 p = 25.98 × 10–3

80

6 3 0

439

Shear 40 0 0.0

0.2

0.4

0.6

0.8

1.0

1.2

1.4

1.6

1.8

2.0

Axial Total Strain ()%

FIGURE 8.9 Stress response to strain path of torsion followed by tension (From Wu, H.C. and Yang, R.J., Int. J. Non-Linear Mech., 18, 395, 1983. With permission from Elsevier).

prestrain in tension. Type 304 stainless steel tubular specimens were tested at constant strain-rate of 5 × 10−4 per second. The theory was capable of predicting the stress response to the two cyclic strain paths considered. Further investigation of multiaxial straining was conducted by Wu et al. [30]. Plastic strain-controlled experiments were conducted on 304 stainless steel tubular specimens. The plastic strain-control was feasible by means of a computer-aided material test system. Three in-phase plastic strain paths (a pure axial path, a pure torsional path, and an axial–torsion in-phase path) and two out-of-phase plastic-strain paths (small and large perturbations from the axial–torsion in-phase path) were studied, and the endochronic constitutive equation (8.125) was used to obtain theoretical results for the ﬁve strain paths considered. It was shown that the theory and experiment have good agreement. Furthermore, both experimental and theoretical results show that strain hardening is enhanced by out-of-phase loading. Figure 8.10(a) shows the theoretical and experimental plastic strain path of path 5, the out-of-phase path with large perturbation from the axial–torsion in-phase path. The corresponding axial stress versus plastic axial strain plot is shown in Figure 8.10(b), and the corresponding shear stress versus plastic shear strain plot is shown in Figure 8.10(c). Finally, we mention that Wu and Yeh [31] applied (8.125) to investigate the combined axial-internal pressure loading of tubular specimens and compared their results with their own experimental data. Additional work on endochronic theory and its application have been conducted by Valanis and his coworkers [32,33] and by Atluri and coworkers in numerical computation [34,35].

© 2005 by Chapman & Hall/CRC Press

440

Continuum Mechanics and Plasticity 1.2 Plastic Shear-Strain (%)

(a)

Reference Experimental D

1

E

0.8 B

0.6 0.4 0.2

C

0 0 A

–0.2 0.0

400

(b)

Experimental Endochronic

300 Axial Stress (MPa)

0.2 0.4 Plastic Axial-Strain (%)

0.6

E C

A

200 100 0 –100

D

B

–200 –300 0.0

(c)

0.2 0.4 Plastic axial-strain (%)

0.6

200

D

Shear Stress (MPa)

B 100 0

0

E A

–100

–200 –0.2

C Experimental Endochronic 0 0.2 0.4 0.6 0.8 Plastic Shear-Strain (%)

1

FIGURE 8.10 Response to zigzag plastic strain path: (a) plastic strain path, (b) axial stress, (c) shear stress (From Wu, H.C. et al., J. Eng. Mater. Technol., 108, 262, 1986. With permission from ASME).

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory 8.4.6

441

The Endochronic Theory of Viscoplasticity

A general introduction of the strain-rate effect is given in Section 5.2.4. The strain-rate sensitive plasticity is also known as the viscoplasticity. Based on the ﬂow theory of plasticity, the viscoplastic effect was investigated by Perzyna [36], Phillips and Wu [37], Krempl [38], and others. The endochronic viscoplasticity provides a framework for a uniﬁed theory to discuss the constant strain-rate stress–strain curves, the creep curves, and the stress relaxation all together. In describing the viscoplastic behavior, Valanis [6] deﬁnes the intrinsic time as dζ 2 = Pijkm dεij dεkm + g2 dt2

(8.152)

where g is a material parameter. The intrinsic time given by (8.49) is a reduced version for strain-rate independent plasticity. The simple endochronic viscoplasticity was applied by Wu and his coworkers [39–41] to study the stress wave propagation for strain-rate sensitive materials. In Wu and Yip [42], the strain-rate and strain-rate history effects on the dynamic behavior of metals were investigated using the improved endochronic theory. Lin and Wu [43] further applied the theory to viscoplastic wave propagation. Furthermore, the theory was applied by Wu and Ho [44] to discuss the phenomenon of transient creep. In this subsection, we discuss the strain-rate effect for uniaxial loading following the work of [42] and creep following [44]. To obtain a more general form of the intrinsic time measure, which accounts for strain-rate, it is assumed that a spectrum of r intrinsic times exists and each intrinsic time corresponds to an internal state variable. Thus, for each intrinsic time, we write dζi2 = hi (ε p )(dε p )2 + gi (ε p )(dt)2 ,

i = 1, 2, . . . , r

(8.153)

where hi and gi are functions of dε p , and t is the real time. (8.153) can be written as gi (ε p ) 1/2 p dε , dζi = ± hi (ε p ) + p 2 (˙ε )

i = 1, 2, . . . , r

(8.154)

Introducing an average intrinsic time measure such that dζ = (dζ1 , dζ2 , . . . , dζr )

(8.155)

then, using (8.154), we obtain dζ = ±k(εp , ε˙ p )dε p

(8.156)

The function k is known as the strain-rate sensitivity function and it is a function of ε p and ε˙ p . For simplicity, we assume that k is a function of ε˙ p

© 2005 by Chapman & Hall/CRC Press

442

Continuum Mechanics and Plasticity

only, that is, dζ = k(˙ε p )|dε p |

(8.157)

This relation is the same as that proposed earlier in [39], except that we now use the plastic strain instead of the total strain. In the three-dimensional version, (8.157) is (dζ )2 = k 2 (|˙ε p |)dεp · dεp

(8.158)

Let us now consider the constant strain-rate stress–strain curves. Using (8.111), form (a) of (8.110), and (8.157), (8.109) may be integrated while holding ε˙ p constant to yield σ = σyD (1 + β1 ε p ) + (σ 0 − σyD )(1 + β1 ε p ){1 − (1 + β1 ε p )−n } + E2 ε p (8.159) where σyD =

σy k(˙ε p )

and

β1 = βk =

(8.160)

and n=

α +1 β

Et − E2 σ0

(8.161)

Note that σy is the static yield stress. The dynamic yield stress σyD , the tangent modulus Et at large εp , and the intercept of the asymptote to the stress–strain curve with the stress axis σ 0 can be measured directly from each constant strain-rate stress–strain curve (see Figure 8.5). For the sake of simplicity, we have not introduced new notations for Et and σ 0 . But these are dynamic quantities and they vary with each constant strain-rate stress–strain curve. For most materials, the constant strain-rate stress–strain curves for various strain-rates are parallel to each other at large ε p and, in this case, Et does not vary with the strain-rate. Using the method of Example 8.2, the relations in (8.161) have been obtained. The parameters β1 , n, and E2 are determined by the trial and error method so that the theoretical curve agrees with the experimental reference curve. The experimental reference curve is usually taken as the constant strain-rate stress–strain curve that has the lowest strainp rate ε˙ 0 of all the curves. The following function has been used by Lin and Wu [39] and Wu and Yip [42] to deﬁne the strain-rate sensitivity function k p

k(˙ε ) = 1 − ks log

© 2005 by Chapman & Hall/CRC Press

ε˙ p p

ε˙ 0

(8.162)

Internal Variable Theory and Endochronic Theory

443

where ks is a material parameter. Figure 8.11 shows that (1.162) can ﬁt nicely to the experimental data of Karnes and Ripperger [45] for annealed high-purity aluminum for the strain-rate range from 10−4 to 103 s−1 . The strain-rate is shown as θ˙ in the ﬁgure. From each experimental constant strain-rate stress– strain curve, we determine the dynamic yield stress σyD , and, since we know σy , k(˙ε p ) can be found from (8.160). Equation (8.159) describes a set of stress–strain curves at various constant strain-rates. By use of (8.162), the theoretical constant strain-rate stress–strain curves thus obtained are compared with the experimental curves of [45] and shown in Figure 8.12. The parameters for theoretical curves are E0 = 10 × 106 psi (6.89 × 104 MPa), σ00 = 1 × 103 psi (6.89 MPa), σy = 0.75 × 103 psi

1

k

0.8 0.6 0.4 0.2 2

4 · ·) Log(/ 0

6

8

Experiment by Karnes and Ripperger [45] · p/ · p) Theory: k = 1 – 0.1165 Log ( 0 FIGURE 8.11 Strain-rate sensitivity function k (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

00

·p = 20

Stress (MPa)

80

·p = 4000

60 40

·p =1000

·p = 500

–2

2 × 10

20 –4 s–1

2 × 10

0

0.5

1.0

1.5

2.0

Plastic Strain (%) FIGURE 8.12 Constant strain-rate stress–strain curves for aluminum (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

444

Continuum Mechanics and Plasticity

(5.17 MPa), β = 180, n = 25, and E2 = 0. We note that σ00 is the intercept of the asymptotic line with the stress axis for the reference stress–strain curve. The foregoing work is relevant to strain-hardening metallic materials such as f.c.c. metals. For materials such as mild steel, strain-softening occurs after initial yielding. However, the material switches from strain softening to strain-hardening at a strain of approximately 2%, and we shall call this type of materials strain softening–hardening materials. The ζ –z relation for this type of materials requires special attention. We use (8.110) form (c) for the strain-softening portion and form (a) for the strain-hardening portion of the material behavior, and introduce a critical intrinsic time ζcr (with the corresponding zcr ) to indicate the point of changeover from softening to hardening in a stress–strain curve. Thus, the following relations apply: dζ = f (z) = e−βs z dz

and ζ =

1 (1 − e−βs z ) βs

with βs > 0,

for z ≤ zcr (8.163)

dζ = bh eβh (z−zcr ) dz

and ζ = ζcr −

bh [1 − eβh (z−zcr ) ] βh

for z ≤ zcr (8.164)

where βs , βh , bh are material parameters. Assuming that the ζ –z relation is smooth and differentiable at the critical point, we have bh = e−βs zcr

(8.165)

Thus, bh can be calculated if βs and zcr are known. The ζ –z relation for strain softening–hardening materials is shown schematically in Figure 8.13. Using the isotropic-hardening function deﬁned by (8.163) to (8.165) and the strain-rate sensitivity function deﬁned by (8.162), (8.109) leads to the constant strain-rate stress–strain curves for mild steel shown in Figure 8.14. The plastic strain-rate is denoted by θ˙ in the ﬁgure. Theoretical results compare favorably with the experimental data of Cambell and Marsh [46] in the

cr

0

zcr

z

FIGURE 8.13 Isotropic-hardening function f for strain softening–hardening materials.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

445

70 Theory

65

Experiment by Cambell and Marsh [46]

60

= 5.0/s–1 · = 3.0 · = 0.5 · = 0.2 · = 0.02 · = 10–4

450

·

400

·

= 5.0

55

·

350 50 MPa

Stress × 103 psi

= 0.5

·

= 0.5 45

·

= 0.2

40

300

·

= 0.02 250 35

·

= 10–4/s–1 30

200 0

1

2

3

4

5

Plastic Strain (%) FIGURE 8.14 Constant strain-rate stress–strain curves for mild steel (From Wu, H.C. and Yip, M.C., Int. J. Solids Struct., 16, 515, 1980. With permission from Elsevier).

range of strain-rate from 10−4 to 5 s−1 . The details of the theoretical work are reported in [42]. Wu and Yip [42] also considered the strain-rate history effect in two loading sequences: the low–high strain-rate change test sequence and the high–low strain-rate change test sequence. In the ﬁrst test sequence, the specimens

© 2005 by Chapman & Hall/CRC Press

446

Continuum Mechanics and Plasticity

were tested initially at a low prescribed constant strain-rate and tested at a higher strain-rate in the subsequent loading. In the second test sequence, the specimens were ﬁrst tested at a high strain-rate and subsequently tested at a lower strain-rate. Both strain-hardening materials and strain softening– hardening materials were investigated. Different test sequences resulted in different subsequent stress–strain behaviors. Lin and Wu [43] used a nonlinear form of (8.162) to describe the strain-rate sensitive behavior of α-titanium. The intrinsic time deﬁned by (8.158) is applicable to describing constant strain-rate stress–strain curves as previously shown. In the uniﬁed theory, (8.158) is combined with (8.152) to yield (dz)2 =

dζ f (ζ )

2

+ g2 dt2

(8.166)

where (dζ )2 = k 2 (|˙ε p |)dε p · dε p

and

k(|˙ε p |) = 1 − ks log

|˙εp | |˙ε p |0

(8.167)

The intrinsic time expressed by (8.166) and (8.167) provides a versatile deﬁnition of intrinsic time. In this way, the strain-rate sensitive plasticity (the rate dependence) can be accounted for by the function k(|˙εp |), and (8.167) shows that the accumulation of ζ is strain-rate dependent. Creep or stress relaxation behavior (the time dependence) is accounted for by the function g. Although both rate dependence and time dependence are time-dependent behaviors, it is convenient to use these terminologies. A ﬂow theory of viscoplasticity can be derived from the endochronic viscoplasticity equations. The method of derivation and the resulting equations are the same as those presented in Section 8.4.4, except that the yield stress is replaced by the dynamic yield stress. The dynamic yield stress is deﬁned by (8.160) through the strain-rate sensitivity function k. The ﬂow rule remains the same as in (8.97), which is dεp =

(σ − α) dz σy

(8.168)

but the yield criterion is now

(σ − α) · (σ − α) =

σy f (z)

2

k

with dζ 2 = 0

(8.169)

or dζ 2 = 0

© 2005 by Chapman & Hall/CRC Press

(8.170)

Internal Variable Theory and Endochronic Theory

447

The function k describes the strain-rate sensitivity of the dynamic loading surface so that σy /k is the size of the constant strain-rate dynamic loading surface, which is also known as the SCISR (surface of constant inelastic strainrate) — an acronym introduced by Robinson [47]. The function f denotes the size of the SCISR due to isotropic hardening and α denotes the location of the center of the SCISR. The distortion of the yield and loading surfaces is not described by (8.169). That subject has been discussed by Wu et al. [48] and Wu and Lu [49]. In the case of time-dependent deformation process (creep or stress relaxation), g = 0; (8.167) and (8.168) may be substituted into (8.166) to obtain dz2 = k 2 (|˙ε p |)

|σ − α|2 2 dz + g2 dt2 (σy f )2

(8.171)

or dz =

g 1 − k 2 (|σ − α|2 /(σy f )2 )

dt

(8.172)

Note that since dz > 0 and dt > 0, it must be that g > 0. Acreep test is preceded by a constant strain-rate test. During this stage of plastic deformation, the stress point is on the yield surface which from (8.169) is σ f (z) σ − α = y k

or

1 − k2

|σ − α|2 =0 (σy f )2

(8.173)

However, since the stress point in the stress space stays at the same point but the back stress increases during creep as experimentally observed by Wu and Ho [50] for annealed 304 stainless steel (there may also be isotropic hardening for other materials), the stress point, which is on the SCISR when creep begins, falls back into the “elastic region” of that SCISR as the SCISR moves during creep. In the case of stress relaxation, the stress point also falls back into the “elastic region” of the SCISR as the stress level reduces. Therefore, during time-dependent inelastic behavior 1 − k2

|σ − α|2 = 0 (σy f )2

(8.174)

In an effort to unify the deﬁnition of intrinsic time for both plastic deformation and time-dependent inelastic behavior, the function g must reduce to zero in the case of plastic deformation. To this end, the following form of g has been

© 2005 by Chapman & Hall/CRC Press

448

Continuum Mechanics and Plasticity

found to be satisfactory g = B 1 − k2

|σ − α|2 (σy f )2

(8.175)

where B is a scaling function. Substituting (8.175) into (8.172), the intrinsic time for time-dependent inelastic behavior is now given by dz = B dt

(8.176)

and the time-dependent inelastic strain (creep) may be found from (8.168) as dσ (σ − α) = B dt 2µ0 σy

dεp = de −

(8.177)

which is rewritten as

dσ = 2µ0

(σ − α) de − B dt σy

(8.178)

In the rate form, (8.178) is

σ˙ = 2µ0

(σ − α) e˙ − B σy

(8.179)

Creep and stress relaxation are now discussed separately. In the case of creep, the stress holds constant, that is, σ˙ = 0, and the creep strain-rate (˙εp )c equals the total strain-rate. Therefore, from (8.179) (˙εp )c = e˙ =

(σ − α) B σy

(8.180)

The form of the scaling function B is now investigated. Miller [51] suggested that the creep rate is a function of kinematic and isotropic hardenings and proposed the expression p

(˙ε )c = ϕ

σ − α R

(8.181)

where R denotes isotropic hardening; σ is the hold stress; and ϕ is a nonlinear function to be further discussed. Thus, during the creep process, both kinematic and isotropic hardenings are active. The form of (8.181) encompasses the experimental observations that both isotropic and kinematic hardenings can be important factors in creep [50]. This equation is, therefore,

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

449

used in this chapter. In classical creep theories and uniﬁed viscoplasticity theories, the power, the exponential, and the hyperbolic sine functions are usually used to provide a description of creep strain. Of these functional forms, the power form has been broadly used because of its numerical simplicity. This function is now used in this writing, so that B=

bσy |σ − α|

k|σ − α| σy f

m (8.182)

where b and m are material parameters. Finally by substituting (8.182) into (8.180), the creep strain-rate is obtained as

k|σ − α| (˙εp )c = b σy f

m

(σ − α) |σ − α|

(8.183)

which is a specials case of (8.181). At the very beginning when creep is about to occur, the stress is still on the loading surface (SCISR) so that, from (8.169), |σ −α| = (σy f )/k, g = 0, and (8.183) does not apply yet. However, only a small perturbation so that |σ −α| < (σy f )/k would start the creep process and make (8.183) applicable. Since the perturbation is small, |σ − α| ≈ (σy f )/k, so that (˙εp )c = b. Therefore, b may be identiﬁed as the initial creep strain-rate. During the process of stress relaxation, the total strain increment de = 0 so that, by use of (8.179), the rate of stress relaxation is σ˙ = −2µ0 B

σ − α σy

(8.184)

Wu and Ho [44] applied the foregoing theory to describe their own experimental results for AISI type 304 stainless steel. Isotropic hardening is insigniﬁcant for this material [52]. It has been shown in [44] that the viscoplastic endochronic constitutive equation is capable of describing the inelastic behavior of this rate-sensitive metal for a variety of loading histories. The features include combined isotropic–kinematic hardening, rate sensitivity of plastic deformation, creep, and stress relaxation. In particular, the creep curves with a constant strain-rate preloading stage previously shown in Figure 5.13 are well predicted. In addition, they found that (1) meaningful results of transient creep can be obtained only from creep tests with a carefully controlled constant strain-rate preloading stage; (2) a correlation between constant strain-rate and constant stress-rate stress–strain curves can be achieved by means of the viscoplastic endochronic constitutive equations; (3) with the same strain-rate in the elastic region, the stress–strain curve of constant stress-rate is stiffer than that of constant strain-rate; (4) a correlation between creep with constant strain-rate and constant stress-rate preloadings can be achieved by means of the viscoplastic endochronic constitutive equations;

© 2005 by Chapman & Hall/CRC Press

450

Continuum Mechanics and Plasticity

and (5) the initial creep rate is a continuation of the strain-rate of preloading and the creep curves are noticeably inﬂuenced by the initial creep rate.

References 1. Valanis, K.C., The viscoelastic potential and its thermodynamic foundation, Iowa State Univ., ERI Report 52, 1967, J. Math. Phys., 48, 262, 1968. 2. Valanis, K.C., Irreversibility and existence of entropy, Int. J. Nonlinear Mech., 6, 337, 1971. 3. Valanis, K.C., Proper tensorial formulation of the internal variable theory, The endochronic time spectrum, Arch. Mech., 29, 173, 1977. 4. Valanis, K.C., A gradient theory of internal variables, Acta Mech., 116, 1, 1996. 5. Valanis, K.C., Irreversible Thermodynamics of Continuous Media, Springer-Verlag, Udine, 1971. 6. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 7. Valanis, K.C., Fundamental consequences of a new intrinsic time measureplasticity as a limit of the endochronic theory, Arch. Mech. 32, 171, 1980. 8. Callen, H.B., Thermodynamics, John Wiley & Sons, New York, 1960, 15. 9. Coleman, B. and Gurtin, M., Thermodynamics of internal state variables, J. Chem. Phys., 47, 599, 1967. 10. Ilyushin, A.A., On the relation between stresses and small strains in continuum mechanics, Prikl. Mat. Mekh., 18, 641, 1954 (in Russian). 11. Pipkin, A.C. and Rivlin, R.S., Mechanics of rate-independent materials, J. Appl. Math. Phys. (ZAMP), 16, 313, 1965. 12. Valanis, K.C. and Wu, H.C., Endochronic representation of cyclic creep and relaxation of metals, J. Appl. Mech., 42, 67, 1975. 13. Wu, H.C. and Lin, H.C., Combined plastic waves in a thin-walled tube, Int. J. Solids Struct., 10, 903, 1974. 14. Lin, H.C. and Wu, H.C., Strain-rate effect in the endochronic theory of viscoplasticity, J. Appl. Mech., 43, 92, 1976. 15. Kosinski, W. and Wu, H.C., On steady viscoplastic waves. Endochronic theory, Bull. L’Acad. Polon. Sci., Ser. Sci. Tech., 26, 109, 1978. 16. Wu, H.C. and Yip, M.C., Finite difference solution for the uniaxial endochronic viscoplastic wave problem, J. Appl. Mech., 45, 221, 1978. 17. Jao, S.Y., Arora, J.S., and Wu, H.C., An optimization approach for materialconstant determination for the endochronic constitutive model, Comput. Mech., 8, 25, 1991. 18. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 19. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 20. Prager, W., The theory of plasticity: a survey of recent achievements (James Clayton Lecture), Proc. Inst. Mech. Eng., 169, 41, 1955.

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

451

21. Ziegler, H., A modiﬁcation of Prager’s hardening rule, Quart. Appl. Math., 17, 55, 1959. 22. Wu, H.C. and Yip, M.C., Endochronic description of cyclic hardening behavior for metallic materials, J. Eng. Mater. Technol., 103, 212, 1981. 23. Lamba, H.S. and Sidebottom, O.M., Proportional biaxial cyclic hardening of annealed oxygen-free high-conductivity copper, J. Test. Evaluation, 6, 260, 1978. 24. Wu, H.C., Aboutorabi, M.R., and Chen, P.C.T., Cyclic torsion of a circular cylinder and its residual stress distribution, J. Eng. Mater. Technol., 107, 48, 1985. 25. Wu, H.C. and Yang, R.J., Application of the improved endochronic theory of plasticity to loading with multi-axial strain-path, Int. J. Non-Linear Mech., 18, 395, 1983. 26. Ohashi, Y., Tokuda, M., and Tanaka, Y., Precise experimental results on plastic behavior of brass under complex loading, Bull. De L’Acad. Polon. Des Sci., Ser. Sci. Tech., 26, 261, 1978. 27. Ohashi, Y., Tokuda, M., Mitake, T., Kurita, Y., and Suzuki, T., Stress–strain relation of integral type for deformation of brass along strain trajectories consisting of three normal straight branches, Archs. Mech., 32, 125, 1980. 28. Ohashi, Y., Tokuda, M., Suzuki, T., and Kurita, Y., Stress–strain relation of brass for the plastic deformation along bi-linear strain trajectories with various corner angles, Bull. Japan. Soc. Mech. Eng., 24, 1909, 1981. 29. Wu, H.C., Yang, C.C., and Chu, S.C., Further application of endochronic constitutive equation to loading with non-proportional axial–torsional strain-path, Int. J. Non-Linear Mech., 20, 41, 1985. 30. Wu, H.C., Yao, J.C., and Chu, S.C., Investigation of endochronic constitutive equation subjected to plastic strain-controlled axial-torsional deformation, J. Eng. Mater. Technol., 108, 262, 1986. 31. Wu, H.C. and Yeh, W.C., Further veriﬁcation of endochronic theory under biaxial load, J. Eng. Mater. Technol., 111, 115, 1989. 32. Valanis, K.C. and Fan, J., Endochronic analysis of cyclic elastoplastic strain ﬁelds in a notched plate, J. Appl. Mech., 50, 789, 1983. 33. Valanis, K.C. and Lee, C.F., Endochronic theory of cyclic plasticity with application, J. Appl. Mech., 51, 367, 1984. 34. Watanabe, O. and Atluri, S.N., A new endochronic approach to computational elastoplasticity: example of a cyclically loaded cracked plate, J. Appl. Mech., 52, 857, 1985. 35. Watanabe, O. and Atluri, S.N., Internal time, general internal variable, and multi-yield-surface theories of plasticity and creep: a uniﬁcation of concepts, Int. J. Plasticity, 2, 37, 1986. 36. Perzyna, P., The constitutive equations for rate sensitive plastic materials, Quart. Appl. Math., 20, 321, 1963. 37. Phillips, A. and Wu, H.C., A theory of viscoplasticity, Int. J. Solids Struct., 9, 15, 1973. 38. Krempl, E., Models of viscoplasticity. Some comments on equilibrium (back) stress and drag stress, Acta Mech., 69, 25, 1987. 39. Lin, H.C. and Wu, H.C., Strain-rate effect in the endochronic theory of viscoplasticity, J. Appl. Mech., 43, 92, 1976. 40. Wu, H.C. and Yip, M.C., Finite difference solution for the uniaxial endochronic viscoplastic wave problem, J. Appl. Mech., 45, 221, 1978.

© 2005 by Chapman & Hall/CRC Press

452

Continuum Mechanics and Plasticity

41. Kosinski, W. and Wu, H.C., On steady viscoplastic waves. Endochronic theory, Bull. L’Acad. Polon. Scien., Ser. Sci. Tech., 26, 109, 1978. 42. Wu, H.C. and Yip, M.C., Strain rate and strain rate history effects on the dynamic behavior of metallic materials, Int. J. Solids Struct., 16, 515, 1980. 43. Lin, H.C. and Wu, H.C., On the rate-dependent endochronic theory of viscoplasticity and its application to plastic-wave propagation, Int. J. Solids Struct., 19, 587, 1983. 44. Wu, H.C. and Ho, C.C., An investigation of transient creep by means of endochronic viscoplasticity and experiment, J. Eng. Mater. Technol., 117, 260, 1995. 45. Karnes, C.H. and Ripperger, E.A., Strain-rate effect in cold worked high-purity aluminum, J. Mech. Phys. Solids, 14, 75, 1966. 46. Cambell, J.D. and Marsh, K.J., The effect of strain-rate on the post-yield ﬂow of mild steel, J. Mech. Phys. Solids, 11, 49, 1963. 47. Robinson, D.N., On thermomechanical testing in support of constitutive equation development for high temperature alloys, NASA CR 174879, 1985. 48. Wu, H.C., Hong, H.K., and Lu, J.K., An endochronic theory accounted for deformation induced anisotropy, Int. J. Plasticity, 11, 145, 1995. 49. Wu, H.C. and Lu, J.K., Further development and application of an endochronic theory accounted for deformation induced anisotrophy, Acta Mech., 109, 11, 1995. 50. Wu, H.C. and Ho, C.C., Strain hardening of annealed 304 stainless steel by creep, J. Eng. Mater. Technol., 115, 345, 1993. 51. Miller, A.K., An inelastic constitutive model for monotonic, cyclic, and creep deformation, J. Eng. Mater. Technol., 98, 97, 1976. 52. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991.

Problems (1) Derive (8.66) and (8.67). (2) Derive (8.71) and (8.72). (3) In the simple endochronic theory, if in the one-dimensional straining the intrinsic time is deﬁned by dζ = ±k dε, where k is a constant, plot the ε versus ζ relation for straining followed by unstraining. (4) For a thin-walled tube made of an initially isotropic material subjected to combined axial–torsion, determine k1 and k2 in the expression dζ 2 = k12 (dεp )2 + k22 (dηp )2 , where ζ is intrinsic time and ηp is the plastic part of the tensorial shear strain. (5) Show that the solution of (8.90) is given by (8.91) and (8.92), if k1 = 1. (6) We consider here the kernel function ξ(z) of the deviatoric constitutive equation (8.82). In Example 8.2, the kernel function is given by two exponential terms. Consider now the case that the kernel function consists of n number of

© 2005 by Chapman & Hall/CRC Press

Internal Variable Theory and Endochronic Theory

453

(b)

(a)

0

60°

FIGURE 8.15 (a) Figure of Problem (8), (b) Figure of Problem (9).

exponential terms, show that in the case of k1 ≈ 1, the deviatoric stress is

σ = 2µ0 where ρ(z) = δ(z) +

z 0

ξ(z − z )

n−1 s

z de dQ dz = 2µ ρ(z − z ) dz 0

dz dz 0

Rs e−αs z + R0 .

(7) In the strain controlled cyclic loading discussed in Section 8.4.5.2, the amplitude of the total strain is kept constant throughout the test. The amplitude of the plastic strain ˜εp becomes constant at stable condition. Let ζ˜ denote the change in ζ in 41 -cycle at the stable condition and the corresponding change in z is ˜z. Show that, if Form (b) of (8.110) is used for the f function, then when z is large ζ˜ /C = ˜z = constant. Show that the cyclic stress–strain curve is σ = σ 0 − (σ 0 − Cσy )

2e−2α˜z 1 + e−2α˜z

+ E2 ε p

(8) In a strain-controlled combined tension–torsion test of a tubular specimen, if the strain-path is linear shown in Figure 8.15(a), use the endochronic constitutive equation to determine the corresponding stress-path. (9) In a stress-controlled combined tension–torsion test of a tubular specimen, consider the tor-ten path shown in Figure 8.15(b). Use the endochronic constitutive equation to determine the corresponding strain-path. Plot the strain-path. (10) In the constant strain-rate uniaxial stress test, if the test is conducted at a low strain-rate into the plastic strain range and then changed to a higher constant strain-rate, what happens to the stress–strain curve?

© 2005 by Chapman & Hall/CRC Press

9 Topics in Endochronic Plasticity

9.1

Introduction

The endochronic theory of plasticity presented in Chapter 8 is further developed in this chapter and applied to investigate topics such as anisotropic plasticity, ﬁnite plastic deformation, engineering materials with plastic volumetric deformation, and damage mechanics. It is seen that the endochronic theory is versatile and is applicable to a wide range of engineering materials.

9.2

An Endochronic Theory of Anisotropic Plasticity

Material anisotropy is a signiﬁcant factor affecting metal forming, and it is of special importance in the case of sheet metals. The anisotropic properties of sheet metals are discussed in Chapter 10 from the viewpoint of the ﬂow theory of plasticity. A general theory of anisotropic plasticity is developed in Chapter 11 using a convected coordinate system. In this section, we discuss the anisotropic plastic behaviors of metals using a endochronic plasticity. We discuss the topic of deformation induced anisotropy and develop an endochronic theory for anisotropic sheet metals.

9.2.1

An Endochronic Theory Accounting for Deformation Induced Anisotropy

In the endochronic theory, the free energy function is from (8.63) given by = 12 ε · A · ε + ε · Br · qr + 12 qr · Cr · qr

(9.1)

The constitutive equation and the evolution equations are from (8.51) and (8.57) σ=

∂ ∂ε

and

r ∂ r dq + b · = 0, ∂qr dz

r = 1, 2, . . . , n

(9.2) 455

© 2005 by Chapman & Hall/CRC Press

456

Continuum Mechanics and Plasticity

where A, Br , Cr , and br are isotropic fourth-rank constant tensors; σ, ε, and qr are symmetric tensors. By use of (9.1) and (9.2), the constitutive equation becomes σkk = 3A0 εkk + σij = A2 eij +

3 Br0 qrkk

r

(9.3)

Br2 pijr

r

To consider deformation induced anisotropy, the evolution of qr must depend on the strain path. This may be achieved by having an anisotropic br . Following Wu and Yeh [1], we deﬁne a strain path with reference to a coordinate system. Thus, we may talk about the normal strain and the shear strain. The internal structure of a material changes differently when it is under normal strain and under shear strain. Hence, qr11 evolves differently than qr12 . We assume that qrij is symmetric and write its components in a matrix form as [qr ] = [qr11 , qr22 , qr33 , qr23 , qr13 , qr12 ]T

(9.4)

We assume further that, in the internal structure, no coupled effect exists either between shear and normal components or among shear components. Then, tensor brijkm is of the following form:

br1 br 2 r b2 r [b ] = 0 0

br2

br2

0

0

br1

br2

0

0

br2 0

br1 0

0 br3

0

0

0

0

0

0

0

0

0 br3

0 0 0 0

0

0

br3

(9.5)

The matrix in (9.5) is obtained by considering symmetry during permutation of 1, 2, and 3. We further have br1111 = br2222 = br3333 = br1 , br2323 = br1313 = br1212 = br3 , other brijkm = 0 br1122 = br1133 = br2233 = br3311 = · · · = br2 ,

(9.6)

We now consider the evolution of qr . Using (9.1), we obtain the following expression ∂ = Br1 εkk δij + Br2 εij + C1r qrkk δij + C2r qrij ∂qrij

© 2005 by Chapman & Hall/CRC Press

(9.7)

Topics in Endochronic Plasticity

457

On the other hand, we have r (b1 − br2 )˙qr11 + br2 q˙ rkk br1 q˙ r11 + br2 q˙ r22 + br2 q˙ r33 br q˙ r + br q˙ r + br q˙ r (br − br )˙qr + br q˙ r 1 2 11 1 22 2 33 2 22 2 kk r r r rq r + br q r r )˙ r + br q r ˙ ˙ ˙ b + b (b − b q q 2 11 2 22 1 33 2 33 2 ˙ kk 1 = br · q˙ r = r r r r b3 q˙ 23 b3 q˙ 23 br3 q˙ r13 br3 q˙ r13

br3 q˙ r12

(9.8)

br3 q˙ r12

Substituting (9.7) and (9.8) into the second equation of (9.2), we obtain the evolution equations for the cases of i = j and i = j. Thus, the governing equations are summarized below. The hydrostatic equations are σkk = 3A0 εkk + 3

Br0 qrkk

r

Br0 εkk

+ C0r qrkk

+ br0

(9.9)

dqrkk =0 dz

and the deviatoric equations are σij = A2 eij +

Br2 pijr

r

Br2 eij + C2r pijr + (br1 − br2 ) Br2 eij + C2r pijr + br3

dpijr dz dpijr dz

= 0,

i=j

= 0,

i = j

(9.10)

It is assumed that the material is plastically incompressible so that only the deviatoric part of the constitutive equation is of further interest. The evolution equations in (9.10) for i = j and i = j can be solved separately to yield expressions for piri (i not summed) and pijr , which are then substituted into the ﬁrst equation of (9.10) to yield σii

z 2 2 e−ρr (z−z ) ei i (z )dz , r C 0 2 r Br Br z 2 2 A2 eij − e−βr (z−z ) eij (z )dz , r C 0 2 r

= A2 ei i −

σij =

Br Br

i not summed (9.11) i = j

where ρr =

© 2005 by Chapman & Hall/CRC Press

C2r , br1 − br2

βr =

C2r br3

(9.12)

458

Continuum Mechanics and Plasticity

By use of Laplace transformation as in Section 8.4.3, (9.11) may be rewritten in terms of plastic strain as

p

σij

=

σy

deij dz

+

z 0

p

de λijkm (z − z ) km dz dz

(9.13)

where

µ

[λ] =

µ

0 µ

ν

ν

0

µ(z) = with

µr e−mr z + µ1

r

ν(z) =

νr e−nr z + ν1

(9.14)

r

ν

in which µr , mr , νr , and nr are material constants of the kernel functions µ(z) and ν(z). Note that in the case of br1 = br2 + br3 , we ﬁnd ρr = βr , which leads to µ(z) = ν(z). Thus, the following endochronic equation for the isotropic rate of kinematic hardening is recovered:

p

σij = σy

deij

+

dz

z 0

p

µ(z − z )

deij dz

dz

(9.15)

We note that the anisotropic form (9.13) is the same as that used by Ohashi and his coworkers [2,3]. Let us further consider the anisotropic endochronic equation (9.13) and, following Wu et al. [4], establish a relation between the deﬁnition of the intrinsic time and the form of the yield function. In (9.13), the back stress is αij =

z 0

p

de λijkm (z − z ) km dz dz

(9.16)

Thus, (9.13) is written as p

σij

− αij =

σy

deij dz

p

=

σy

f (z)

deij dζ

(9.17)

resulting in the following ﬂow rule p

deij =

1 (σ − αij ) dz σy ij

(9.18)

Deﬁne the intrinsic time as dζ 2 = dep · K · dep

© 2005 by Chapman & Hall/CRC Press

(9.19)

Topics in Endochronic Plasticity

459

in which K is a fourth-rank tensor. Then, by using (9.18), (9.19) becomes dζ 2 = (σ − α)

dζ dζ · K · (σ − α) σy f σy f

(9.20)

or [(σ − α) · K · (σ − α) − (σy f )2 ]dζ 2 = 0

(9.21)

Therefore, Either (σ − α) · K · (σ − α) = (σy f )2 or

dζ = 0

with dζ 2 = 0

elastic behavior

(9.22)

The ﬁrst equation of (9.22) is the yield criterion of this anisotropic version of the endochronic plasticity and the second equation of (9.22) describes the elastic behavior, which may be seen from (9.19) due to the positive deﬁniteness of K. The condition dζ = 0 leads to the elastic constitutive equation as in (8.104). p From (9.19), due to the symmetry of deij , Kijkm enjoys the following symmetry: p

p

p

p

deij Kijkm dekm = dekm Kkmij deij , Kijkm = Kkmij = Kijmk

p

p

p

p

deij Kijkm dekm = deij Kijmk demk ,

(9.23)

The number of independent components of K is reduced from 81 to 21. In most previous investigations, K was assumed to be isotropic throughout the course of deformation for mathematical simplicity. This assumption is now relaxed so that K depends on the direction of loading. Equation (9.19) simply asserts that the rate of accumulation of the intrinsic time ζ is not the same when the material is subjected to shear or subjected to tension. However, K is initially isotropic for initially isotropic materials. In which case, the ﬁrst equation of (9.22) reduces to the Mises yield criterion. Equation (9.22) represents a distortion from the Mises yield criterion due to the presence of K. This criterion may be used for the initial as well as the subsequent yielding. In particular, (9.22) can accommodate the idea that the initial yield surface is of the type of Mises, but the subsequent yield surfaces are obtained by the compression and stretching of the Mises yield surface. It should also be pointed out that while the plastic strain increment is still given by (9.18) in this modiﬁed theory, this tensor is no longer normal to the yield surface when K is not isotropic. An important point to make here is that a formal link between the deﬁnition of intrinsic time and the form of the yield function has been established. The deﬁnition of intrinsic time directly affects the form of the yield function, so that

© 2005 by Chapman & Hall/CRC Press

460

Continuum Mechanics and Plasticity

the intrinsic time deﬁned by (9.19) leads to a yield function deﬁned by (9.22). On the other hand, a slightly different deﬁnition of intrinsic time, such as dζ 2 = dεp · K · dεp + tr(L · dεp ) dζ

(9.24)

would lead to a yield function given by (σ − α) · K · (σ − α) + σy f (z) tr[L · (σ − α)] = (σy f (z))2

(9.25)

where L is a material tensor. Explicit equations can be obtained from the theory of this subsection in the case of axial–torsion loading of a thin-walled tubular specimen. Since the material is assumed to be plastically incompressible and the cylindrical coordinates (r, θ , z) are used in this discussion, the conditions p p p p p dεzz + dεrr + dεθθ = 0 and dεrr = dεθθ apply. The latter condition is a good approximation in the case of small plastic deformation, but it is not so when plastic deformation is large; see Wu et al. [5] for further discussion. The matrices of the deviatoric stress σ , the back stress α, and the plastic strain increment dεp are −σ

3 [σ ] = 0 0 −dε p 2 [dεp ] = 0 0

0 −σ 3 τ

−α

0

τ , 2σ 3 0

−dε p 2 dηp

3 [α] = 0 0

zz

0 −αzz 3 αθz

0

αθz , 2αzz 3

0 p dη dε p

(9.26)

which may also be written as column vectors as

−σ 3 2σ , [σ ] = 3 τ

−αzz 3 2α [α] = zz , 3 αθz

−dε p

2 [dεp ] = dε p

(9.27)

dηp

Then, the fourth-rank tensor K is given by the square matrix

K11 [K] = K12 K13

© 2005 by Chapman & Hall/CRC Press

K12 K22 K23

K13 K23 K33

(9.28)

Topics in Endochronic Plasticity

461

Substituting (9.27) and (9.28) into (9.19), we obtain dζ 2 = dεp · K · dεp = K1 (dε p )2 + 2K3 (dε p )(dηp ) + K2 (dηp )2

(9.29)

where K1 =

K11 − K12 + K22 , 4

K2 = K33 ,

K3 =

1 (2K23 − K13 ) 2

(9.30)

and, by using (9.18), the yield function (9.22) becomes 4 9 K1 (σ

− αzz )2 + 43 K3 (σ − αzz )(τ − αθz ) + K2 (τ − αθz )2 = (σy f (z))2

(9.31)

It can be seen from (9.31) that the yield function is an ellipse in the σ versus τ space. As plastic deformation occurs, the ellipse will change its shape, depending on the values of K1 and K2 , when the semimajor and semiminor axes change their lengths. At the same time, isotropic hardening takes place according to function f (z) and the ellipse translates according to the magnitude of the back stress α. In addition, rotation of the yield surface occurs according to the value of 2K3 . Therefore, the major features of subsequent yield surfaces as observed experimentally by Phillips and Tang [6] and Wu and Yeh [7] can all be described. From the experimental results of Phillips and his coworkers, the initial value of K3 is zero. Then by comparing equation (9.31) with the Mises yield criterion, the initial values of K1 and K2 are determined to be 3/2 and 2, respectively. Wu and Lu [8] have established a procedure to determine the metric of the anisotropic intrinsic time using information related to the yield surface of 304 stainless steel.

9.2.2

An Endochronic Theory for Anisotropic Sheet Metals

The contents of this section were initially presented by Wu and Hong [9] and are reproduced here with permission from Elsevier. In the Helmholtz formulation, the free energy is =

1 r A (εij − qrij )(εkm − qrkm ) 2 r ijkm

(9.32)

where Arijkm are constants. For a rolled metal sheet, let x denote the rolling direction (RD), y the transverse direction (TD), and z the normal direction (ND). The nonzero strain components are εx , εy , εxy , and εz . No energy is stored due to εz . Thus, (9.32) reduces to =

1 r [A (εx − qrx )2 + Br (εy − qry )2 + 2Dr (εxy − qrxy )2 2 r + 2Cr (εx − qrx )(εy − qry )]

© 2005 by Chapman & Hall/CRC Press

(9.33)

462

Continuum Mechanics and Plasticity

where Ar , Br , Cr , and Dr are constants. The stress components are

σx = σy = σxy =

∂ = [Ar (εx − qrx ) + Cr (εy − qry )] ∂εx r

(9.34a)

∂ = [Br (εy − qry ) + Cr (εx − qrx )] ∂εy r

(9.34b)

∂ = [Dr (εxy − qrxy )] ∂εxy r

(9.34c)

and the evolution equations for the internal variables are from (8.57): dqrkm ∂ r =0 + b ijkm ∂qrij dz

(r not summed)

(9.35)

In the rolled sheet metal, the components of internal variables are (qrx , qry , qrxy ) and it is assumed that there are no coupling effects among these components, so that the dissipation tensor has the following form

brx

[br ] = 0 0

0 bry 0

0 0 brxy

(9.36)

Using (9.33) and (9.36), (9.35) reduces to dqrx + Pr qrx + U r qry = Pr εx + U r εy dz dqry + Qr qry + V r qrx = Qr εy + V r εx dz dqrxy + Rr qrxy = Rr εxy dz

(9.37a) (9.37b) (9.37c)

where

Pr =

Ar , brx

Ur =

© 2005 by Chapman & Hall/CRC Press

Cr , brx

Qr =

Br , bry

Vr =

Cr , bry

Rr =

Dr brxy

(9.38)

Topics in Endochronic Plasticity

463

Note that (9.37a,b) are coupled in qrx and qry . A standard procedure may be used to decouple the equations. The resulting equations are d¯qrx ˜ r εy + λr1 q¯ rx = C˜ r εx + D dz d¯qry + λr2 q¯ ry = E˜ r εx + F˜ r εy dz

(9.39a) (9.39b)

r r

r where λr1 and λr2 are eigenvalues of the matrix VP r U Qr . Note that since U = 0 r r r and V = 0, there are always two real eigenvalues. q¯ x and q¯ y are related to qrx and qry through the eigenvectors of the matrix by the following relations qrx = U r (¯qrx + q¯ ry ),

qry = (−Pr + λr1 )¯qrx + (−Pr + λr2 )¯qry

(9.40)

and [−(Pr )2 + λr2 Pr − Pr V r + λr1 V r ] U r (λr2 − λr1 ) [−Pr U r + λr2 U r − Pr Qr + λr1 Qr ] ˜r = D U r (λr2 − λr1 ) (U r Pr + U r V r ) E˜ r = U r (λr2 − λr1 ) C˜ r =

(9.41)

[(U r )2 + U r Qr ] F˜ r = U r (λr2 − λr1 ) Note that (9.39a,b) are now decoupled in q¯ rx and q¯ ry . These equations may be integrated with results substituted into (9.40) to obtain qrx = U r

z 0

r

+U qry

z

r

= (−P

0 r

˜ r εy (z )]dz e−λ1 (z−z ) [C˜ r εx (z ) + D r e−λ2 (z−z ) [E˜ r εx (z ) + F˜ r εy (z )]dz

+ λr1 )

z

0

r ˜ r εy (z )]dz e−λ1 (z−z ) [C˜ r εx (z ) + D

+ (−Pr + λr2 )

(9.42a)

0

z

e−λ2 (z−z ) [E˜ r εx (z ) + F˜ r εy (z )]dz r

(9.42b)

Also, (9.37c) may be integrated to yield qrxy = Rr

© 2005 by Chapman & Hall/CRC Press

z 0

e−R (z−z ) εxy (z )dz r

(9.42c)

464

Continuum Mechanics and Plasticity

with qrx (0) = qry (0) = qrxy (0) = 0. By substitution of (9.42) into (9.34) and by use of integration by parts, the following expressions are found

dε dεx r ˜ r y dz e−λ1 (z−z ) C˜ r + D dz dz 0 r

z dεy dεx r Nr (9.43a) e−λ2 (z−z ) E˜ r + F˜ r dz + dz dz 0 r

σx = Y1 εx (z) + Y2 εy (z) +

Mr

dε dεx r ˜ r y dz e−λ1 (z−z ) C˜ r + D dz dz 0 r

z (9.43b) r −λr2 (z−z ) ˜ r dεx r dεy ˜ L E dz e +F + dz dz 0 r

σy = Y3 εy (z) + Y4 εx (z) +

σxy =

z

D

r

z

Kr

z

r 0

r dεxy e−R (z−z ) dz dz

(9.43c)

where

˜r − Mr C˜ r − N r E˜ r , Y2 = C − Mr D N r F˜ r r r r r ˜r − Y3 = B − Kr D Lr F˜ r , Y4 = C − K r C˜ r − Lr E˜ r r r r r A= Ar , B = Br , C = Cr ,

Y1 = A −

r

1 = r Ar U r + Cr (−Pr + λr1 ) , λ1

1 r K = r Cr U r + Br (−Pr + λr1 ) , λ1

Mr

r

r

1 = r Ar U r + Cr (−Pr + λr2 ) λ2

1 r r r L = r C U + Br (−Pr + λr2 ) λ2 (9.44)

Nr

Note that all quantities given in (9.44) are constants. A special case of (9.43) is used to derive the following equations

dεy dεx G(z − z ) (H + F) + H dz dz dz 0

z dεy dεx σy = K −3/2 G(z − z ) (G + H) + H dz dz dz 0

z M dεxy σxy = K −3/2 dz Gxy (z − z ) N dz 0 σx = K −3/2

© 2005 by Chapman & Hall/CRC Press

z

(9.45)

Topics in Endochronic Plasticity where

465

r G(z) = Gr e−λ z r r −λrxy z Gxy (z) = Gxy e r

K = 23 (F + G + H)

Gr = 1 r r with Gxy (0) = Gxy =1

with G(0) =

(9.46)

r

and

M = (H + F)(G + H) − H 2

Constitutive equations (9.45) are suitable for use in sheet metals. These are expressions for the stress components in terms of the histories of the total r , λr , and strain components εx , εy , and εxy . In the equations, E, F, G, H, Gr , Gxy r λxy are constants with r = 1, . . . , n. The derivation of (9.45) is given in [9]. It is now desirable to express the stress in terms of the histories of plastic p p p strain components εx , εy , and εxy so that p z p dε dε y x σx = K −3/2 ρ(z − z ) (H + F) + H dz dz dz 0 p z p dεy dεx −3/2 (9.47) σy = K ρ(z − z ) (G + H) + H dz dz dz 0 z p M dε x dz σxy = K −3/2 ρxy (z − z ) N dz 0 The forms of expressions in the square brackets on the right-hand side of (9.45) and (9.47) are assumed to be the same. These forms are established based on plastic deformation for sheet metals, which is further discussed in Chapter 10. The coefﬁcients F, G, H, M, and N are those of the yield function initially proposed by Hill [10]. The kernel functions ρ(z) and ρxy (z) can be determined from knowledge of G(z) and Gxy (z) using the method of Laplace transformation discussed in Section 8.4.3. Omitting the details of derivation, which may be found in [9], the kernel functions are ρ(z) = δ(z) + ρ1 (z)

with ρ1 (z) =

n−1

Rr e−µr z

r=1 n−1

ρxy (z) = δ(z) + ρxy1 (z)

with ρxy1 (z) =

(9.48) r Rxy e−µxyr z

r=1

where µr , and µxyr are positive constants. Substituting (9.48) into (9.47), the constitutive equations for sheet metals may be obtained: Rr ,

r , Rxy

σx = K −3/2

p

p

dεy dεx (H + F) +H dz dz

+ K −3/2

© 2005 by Chapman & Hall/CRC Press

z

0

p

p

dεy dεx ρ1 (z − z ) (H + F) + H dz dz

dz

(9.49a)

466

Continuum Mechanics and Plasticity σy = K

p

z

Denoting

p

dεy

p

dεx ρ1 (z − z ) (G + H) + H +K dz dz 0 z p M dεx dz = K −3/2 + K −3/2 ρxy1 (z − z ) N dz 0 −3/2

σxy

p

dεy

dεx (G + H) +H dz dz

−3/2

dz

p p dεy dεx ρ1 (z − z ) (H + F) + H dz αx = K dz dz 0 p z p dεy dεx −3/2 αy = K ρ1 (z − z ) (G + H) + H dz dz dz 0 z p M dεx αxy = K −3/2 dz ρxy1 (z − z ) N dz 0 −3/2

(9.49b)

(9.49c)

z

(9.49a,b) may be further written as p p dεy dεx +H = (H + F) dζ dζ p p dεy dεx +H = (G + H) dζ dζ

(9.50)

σx − αx K −3/2 f σy − αy K −3/2 f

(9.51)

which may then be solved for p

M

(G + H)(σx − αx ) H(σy − αy ) dεx = − dζ K −3/2 f K −3/2 f p

M

dεy dζ

=

(H + F)(σy − αy ) H(σx − αx ) − K −3/2 f K −3/2 f

(9.52a) (9.52b)

Also, (9.49c) is rewritten as p

σxy − αxy M dεxy = N dζ K −3/2 f

(9.52c)

Therefore, in an anisotropic sheet, it takes a multiaxial stress state to produce a single plastic strain component. Equations (9.52) may be viewed as the ﬂow rule using the concept of the ﬂow theory of plasticity. It may be easily

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

467

shown that the plastic strain increment as given by (9.52) is normal to the yield surface to be discussed in the next paragraph. We note that, in the theory of Section 9.2.1, the plastic strain increment is necessarily pointing along the radial direction, emanating from the center of the yield surface, and it is not normal to the yield surface after the yield surface has suffered a distortion. Finally, plastic incompressibility is assumed so that p

p

p

dεx + dεy + dεz = 0

(9.53)

It was established in [4] that the deﬁnition of the intrinsic time determines the form of the yield function. For sheet metals, we now show that the proposed deﬁnition of intrinsic time leads to Hill’s 1948 quadratic yield criterion. The intrinsic time is deﬁned using the concept of equivalent plastic strain increment discussed in the appendix of [9], that is, dζ = d¯ε =

(G + H) p p [(H + F)dεx + Hdεy ]2 K3

2H p p p p [(H + F)dεx + Hdεy ][(G + H)dεy + Hdεx ] K3 1/2 (H + F) 2N M p 2 p p 2 + [(G + H)dεy + Hdεx ] + 3 dεxy N K3 K

−

(9.54)

Upon substitution of ﬂow rule (9.51) or (9.52), we obtain from (9.54)

σy − α y σx − α x 2 2H σx − αx − K −3/2 f K 3 K −3/2 f K −3/2 f (H + F) σy − αy 2 2H σxy − αxy 2 + 3 − 1 dζ 2 = 0 + K3 K −3/2 f K K −3/2 f

(G + H) K3

(9.55)

Thus, either dζ = 0 and the quantity in the bracket { } = 0, or dζ = 0 and the bracket { } = 0. The cases of dζ = 0 and dζ = 0 correspond to the elastic and plastic behavior, respectively. In the latter case, after simpliﬁcation, we obtain (G + H)(σx − αx )2 − 2H(σx − αx )(σy − αy ) + (H + F)(σy − αy )2 + 2N(σxy − αxy )2 = f 2

(9.56)

This is an extended version of Hill’s yield criterion [10]. The isotropic hardening is expressed by f and the kinematic hardening is expressed by αx , αy , and αxy . Coefﬁcients F, G, H, and N are determined from experiments that p p together with the plastic strain ratio Rα = dεy /dεz are discussed further in Chapter 10. The plastic strain ratio is related to the test of a sheet type tension

© 2005 by Chapman & Hall/CRC Press

468

Continuum Mechanics and Plasticity

specimen, where x is along the longitudinal direction of the specimen, y is the transverse direction, and z = z. Show that the ﬂow rule given by (9.52) obeys the normality rule and is normal to the yield surface given by (9.56).

EXAMPLE 9.1

Solution The yield function from (9.56) is 2φ = (G + H)(σx − αx )2 − 2H(σx − αx )(σy − αy ) + (H + F)(σy − αy )2 + N(σxy − αxy )2 + N(σyx − αyx )2 − f 2

(a)

Let us perform the following partial differentiation ∂φ = (G + H)(σx − αx ) − H(σy − αy ) ∂σx ∂φ = −H(σx − αx ) + (H + F)(σy − αy ) ∂σy

(b)

∂φ = N(σxy − αxy ) ∂σxy Comparing (b) with (9.52), we see that the two sets of equations differ only by a scalar multiple factor. Therefore, we may conclude that (9.52) satisﬁes the normality condition.

9.3

Endochronic Plasticity in the Finite Strain Range

In [11], Valanis considered internal variables qr (r = 1, 2, . . . , n) as quantities which transform as tensors with rotation of the material coordinate system, but remain invariant with rotation of the spatial system. In [12], these variables were regarded as quantities that transform as tensors with rotation of the spatial coordinate system, giving rise to a spatial formulation of the thermodynamics of internal variables. For tensors in the material coordinate system, care was taken to distinguish between the covariant, contravariant, and mixed components. This distinction gave rise to different constitutive equations depending on which components were chosen as independent variables. Valanis [13] further investigated the stress rate and the rate of evolution for the back stress, and recommended that the convected rates be used. He distinguished the convected rate for covariant stress from that for contravariant stress, and applied them to show that, by use of the convected rates, Prager’s linear kinematic-hardening rule did not lead to an oscillatory shear stress–strain curve under simple shearing. It is well known

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

469

that the shear stress–strain curve oscillates when the Jaumann rate is used (Section 7.6.3). Valanis [13] further mentioned that while the two convected rates have clear and distinct physical meanings, the Jaumann rate is the average of the aforementioned two rates and the physical meaning is obscure. The convected rates are further discussed in Chapter 11 in conjunction with the curvilinear coordinate system. While the use of a convected rate is most appropriate for stress and kinematic variables, the use of a convected rate for the back stress is questionable. The back stress is a way to represent anisotropy resulting from the change of material texture due to plastic deformation. While Dafalias [14] uses the concept of plastic spin to account for the change of material texture (see Section 7.6.2), he cautions against associating the plastic spin with the general kinematics of deformation. The concept of plastic spin has been introduced into the endochronic theory by Im and Atluri [15] and Wu et al. [5]. We follow [5] in the remaining part of this section. We ﬁrst discuss the concept of a corotational integral, which is useful in the ensuing discussion of endochronic theory for large strain.

9.3.1

Corotational Integrals

Suppose that a ﬂexible body moves in space. The triad of unit vectors of frame x¯ i that rotates with the body coincides with that of the reference frame xi at time zero. The two sets of coordinates are related by

[¯x] = [M]T [x]

(9.57)

where [M] is the matrix of an orthogonal tensor, such that [M][M]T = [I]. Then, the following transformation laws apply [¯g] = [M]T [g] ¯ = [M]T [T][M] [T]

[g] = [M][¯g] T ¯ [T] = [M][T][M]

(9.58)

where [g] is the matrix of a ﬁrst-rank tensor and [T] is the matrix of a ¯ refer to the x¯ i frame and we may write their second-rank tensor; [¯g] and [T] corotational derivatives as ∇

g = [˙g] − [][g],

∇

˙ − [][T] + [T][] T = [T]

(9.59)

where T ˙ [] = [M][M]

© 2005 by Chapman & Hall/CRC Press

(9.60)

470

Continuum Mechanics and Plasticity

and a dot over a tensor denotes its material derivative. It is easy to show that · ∇

˙¯ T = [M][M]T [T][M][M]T T = [M][T][M]

(9.61)

The expressions of (9.61) show that the corotational rate of T with respect to the reference frame xi is obtained by ﬁnding the material rate of T¯ with respect to frame x¯ i and then transporting the result back to the reference frame xi . It may be shown that the corotational rate is objective by considering a superposed rigid body rotation Q, such that [M ] = [Q][M]. Thus, ¯ = [QM]T [T ][QM] = [M]T [Q]T [T ][Q][M] = [M]T [T][M] [T]

(9.62)

The last expression of (9.62) is obtained from (9.58) and we conclude from (9.62) that [T ] = [Q][T][Q]T

(9.63)

Therefore, by using the ﬁrst expression of (9.61), we obtain

∇

T

∇

∇

˙ T T ¯ = [M ][T][M ] = [Q][M] [M] T [M] [M]T [Q]T = [Q] T [Q]T

(9.64) which shows that the corotational rate is objective. Let us now consider the integral {T} of the second-order objective tensor T [16,17], which is a function of t and t , that is, T = T(t, t ). Here, t is the current time and t is a dummy parameter of integration. Referring to the corotational frame x¯ i , the integral is deﬁned as: ¯ = {T}

t 0

¯ t )]dt = [T(t,

t 0

[M(t )]T [T(t, t )][M(t )]dt = [M(t)]T {T}[M(t)] (9.65)

with {T} = [M(t)]

t 0

[M(t )]T [T(t, t )][M(t )]dt [M(t)]T

(9.66)

The integral {T} is known as the corotational integral. Physically, the corotational integral ﬁrst transfers the tensor T to the x¯ i frame to obtain T¯ and, after integration in the x¯ i frame, it transports the result back to the xi frame. Note that T(t ) is a special case of T(t, t ).

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

471

Let us consider the expression of the back stress α, which will be used later. Let the expression of back stress α for small deformation be α=

z

0

µ(z − z )

dεp dz dz

(9.67)

where z is the intrinsic time. We now extend expression (9.67) to large deformation by use of (9.66). The integrand of (9.67) is a second-order tensor, which becomes tensor µ(z − z )D/˙z in the case of large deformation. Then α is the corotational integral {µ(z − z )D/˙z}. It follows from (9.66) that [α] = [M(z)]

z 0

[M(z )]T [D][M(z )] µ(z − z ) dz [M(z)]T z˙

(9.68)

On the other hand, by use of (9.61), we obtain the corotational rate of α as ∇

T ˙¯ α = [M][α][M]

(9.69)

We further determine α˙¯ as follows ˙¯ = [α]

d[α] ¯ d[α] ¯ dz d[α] ¯ = = z˙ dt dz dt dz

(9.70)

Note that the dot represents material differentiation. In the study of constitutive equations, α is not a function of xi and, therefore, the material differentiation is the same as the ordinary differentiation. From (9.58) and (9.68), we obtain [α] ¯ = [M]T [α][M] =

z 0

µ(z − z )

[M(z )]T [D][M(z )] dz z˙

(9.71)

The derivative of (9.71) with respect to z is [dα] ¯ [M(z)]T [D][M(z)] = µ(0) + dz z˙

z 0

dµ(z − z ) [M(z )]T [D][M(z )] dz z˙ dz (9.72)

By substituting (9.72) and (9.70) in (9.69), we obtain the corotational rate of α as z ∇

dµ(z − z ) [M(z )]T [D][M(z )] [D] T α˙ = z˙ µ(0) dz [M] + [M] dz z˙ z˙ 0 (9.73)

© 2005 by Chapman & Hall/CRC Press

472

Continuum Mechanics and Plasticity

EXAMPLE 9.2

Show that the corotational integral {T} is objective.

Solution We consider a superposed rigid-body rotation Q, such that [M ] = [Q][M]. With reference to the primed system, (9.65) is written as ¯ = {T}

0

t

¯ t )]dt = [T(t,

t 0

[M (t )]T [T (t, t )][M (t )]dt = [M (t)]T {T }[M (t)] (a)

which can be rewritten as {T } = [M (t)]

t 0

[M (t )]T [T (t, t )][M (t )]dt [M (t)]T

t = [Q(t)][M(t)] [M(t )]T [Q(t )]T [Q(t )][T(t, t )][Q(t )]T 0

× [Q(t )][M(t )]dt [M(t)]T [Q(t)]T = [Q(t)][M(t)]

t 0

[M(t )]T [T(t, t )][M(t )]dt [M(t)]T [Q(t)]T

= [Q(t)]{T}[Q(t)]T

(b)

Equation (b) shows that the corotational integral {T} is objective. EXAMPLE 9.3 ∇

Show that the corotational integration of the corotational

derivative T recovers the original tensor T, if T = T(t ), that is, T is not a function of t. Solution From (9.66) and using the ﬁrst equation of (9.61), the corotational integral ∇

of T is ∇ T = [M(t)]

0

= [M(t)]

t

t 0

∇

[M(t )]T T (t ) [M(t )]dt [M(t)]T

˙¯ )]dt [M(t)]T = [M(t)][T][M(t)] T ¯ [T(t = [T]

(a)

Equation (a) demonstrates that the corotational integral of a corotational rate of a tensor is the tensor itself. Therefore, the corotational integral is the inverse operation of the corotational derivative.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity EXAMPLE 9.4

473

Consider the integral for small deformation given by α=

z 0

µ(z − z )

dεp dz dz

(a)

In the case of µ(z) = µ0 e−λz , where µ0 and λ are constant parameters, the differentiation of (a) gives rise to α˙ = µ0 ε˙ p − λα˙z

(b)

In the case of µ(z) = µ1 e−λz + µ2 , where µ(0) = µ1 + µ2 , µ1 , µ2 , and λ are constant parameters, the differentiation of (a) gives rise to α˙ = µ(0)˙εp − λα˙z + λµ2 z˙ εp

(c)

Extend (a) to large deformation and determine the corotational rates. Solution

For the case of µ(z) = µ0 e−λz , dµ(z−z )/dz = −λµ0 e−λ(z−z ) , (9.73) becomes z T ∇

) [M(z )] [D][M(z )] −λ(z−z T α = µ(0)[D] + z˙ [M] (−λ)µ0 e dz [M] z˙ 0 = µ0 [D] − λ˙z[α]

(d)

Note that (d) is in the same form as (b). When µ(z) = µ1 e−λz + µ2 , then from (9.68) [α] = [M(z)]

z

0

µ1 e

+ [M(z)]

z 0

−λ(z−z ) [M(z

)]T [D][M(z )]

z˙

dz

[M(z)]T

[M(z )]T [D][M(z )] µ2 dz [M(z)]T z˙

= [α](1) + [α](2)

(e)

where (1)

[α] [α]

(2)

= [M(z)] = [M(z)]

© 2005 by Chapman & Hall/CRC Press

z 0 z 0

µ1 e

−λ(z−z ) [M(z

)]T [D][M(z )]

z˙

dz

[M(z )]T [D][M(z )] µ2 dz [M(z)]T z˙

[M(z)]T (f)

474

Continuum Mechanics and Plasticity

The integral on the right-hand side of (9.73) is

dµ(z − z ) [M(z )]T [D][M(z )] dz [M]T z˙ dz 0 z T −λ(z−z ) [M(z )] [D][M(z )] = −λ[M(z)] µ1 e dz [M(z)]T = −λ[α](1) z˙ 0 (g)

[M]

z

Substituting (g) into (9.73), we obtain ∇

α = µ(0)[D] − λ[α](1) z˙ = µ(0)[D] − λ[α]˙z + λ[α](2) z˙

(h)

The corotational derivative (h) is not quite of the same form as (c).

9.3.2

Endochronic Equations for Finite Plastic Deformation

In the small strain range, the endochronic constitutive equation is from (8.93) and (8.125) σ = σy

dεp + dz

z 0

dεp dz dz

(9.74)

dζ = f (z) dz

(9.75)

µ(z − z )

The intrinsic time is dζ 2 = dεp · dεp

with

The following yield function may be derived (σ − α) · (σ − α) = (σy, f (z))2

(9.76)

with the ﬂow rule given by dεp =

dz (σ − α) σy

(9.77)

where f (z) is the isotropic hardening function and α is the back stress given by α=

z 0

µ(z − z )

dεp dz dz

(9.78)

This set of equations will now be extended to the ﬁnite strain range by use of stress and strain measures for ﬁnite deformation, the concept of corotational derivative and corotational integral, and the concept of constitutive

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

475

spin (Section 7.6.2). To this end, (9.75) and (9.77) are written as ζ˙ 2 = Dp · Dp

(9.79)

1 (σ − α)˙z σy

(9.80)

Dp =

We extend (9.78) to large deformation by use of (9.66) and the resulting equation, (9.68), is α = M(z) ·

MT (z ) · Dp · M(z ) µ(z − z ) dz · MT (z) z˙

z

0

(9.81)

The integration in (9.81) is with respect to z , which is not t as in (9.66). The intrinsic time z is a monotonically increasing parameter and it does not change during elastic deformation or rigid-body rotation. In general, M(z) is not a unique function of z, because rotation may continue even when z is not changing. This multivalued association of M(z) to z does not invalidate the meaning of integral (9.81), as pointed out by Dafalias [17]. For simplicity in the subsequent calculations, we consider µ(z) = µ1 exp(−λz) + µ2

(9.82)

The corresponding corotational rate of α has been found in Example 9.5 to be ∇

α = (µ1 + µ2 )Dp − λα˙z + λα(2) z˙

(9.83)

where (2)

α

= µ2 M(z) ·

z 0

MT (z ) · Dp · M(z ) dz · MT (z) z˙

(9.84)

Equation (9.83) is the evolution equation of the back stress in terms of the plastic strain rate Dp , the back stress α, and the intrinsic time z. Note that (9.83) is in the incremental form, except for α(2) , which is represented by an integral in (9.84). It is shown in the next section that in solving the problem of a thin-walled tube under torsion, this integral may be integrated so that (9.83) becomes a truly incremental form. The plastic spin, from (7.100), may be written as Wp =

© 2005 by Chapman & Hall/CRC Press

C1 ζ˙ (α · σ − σ · α) (σy f (z))2

(9.85)

476

Continuum Mechanics and Plasticity

where C1 is dimensionless and is a scalar function of the isotropic invariants of σ and α. Using the second expression of (9.75) and the ﬂow rule (9.80), (9.85) becomes C1 f (z)˙z (α · σ − α2 + α2 − σ · α) (σy f (z))2 C1 (σ − α)˙z (α − σ )˙z = + ·α α· σy f (z) σy σy

Wp =

=

C1 (α · Dp σy f (z)

− Dp · α) = K(α · Dp − Dp · α)

with K =

C1 σy f (z) (9.86)

The above expression is the same as (7.101). Equation (9.86) together with (7.138) is substituted into (9.83) when the corotational rate is used in the calculation. 9.3.3

Application to a Rigid-Plastic Thin-Walled Tube Under Torsion

In the consideration of a thin-walled tube under torsion in the large strain range, the elastic strain is neglected, so that the condition of plastic incompressibility is represented by ε˙ r + ε˙ θ + ε˙ z = 0

(9.87)

where ε˙ r denotes the plastic strain-rate in the radial direction; ε˙ θ denotes the plastic strain-rate in the tangential direction; and ε˙ z denotes the plastic strainrate in the axial direction of the tube. The plastic shear strain 2η is related to the angle of twist per unit length ϕ by 2η = rϕ

(9.88)

in which r is the outer radius of the tube. The rate of deformation and spin tensors are expressed as

ε˙ r [Dp ] = 0 0

0 ε˙ θ η˙

0 η˙ , ε˙ z

0 [W ] = 0 0

0 0 −η˙

0 η˙ 0

(9.89)

The equations in (9.89) are now used to derive the explicit expressions for plastic spin and back stress. Let the back stress be symmetric so that

αrr [α] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 αθθ αθz

0 αθz αzz

(9.90)

Topics in Endochronic Plasticity

477

Then, since Dp and α are symmetric, we note that Dp ·α = (α·Dp )T . Therefore, α · Dp − Dp · α 0 0 0 0 (αθθ − αzz )η˙ + αθz (˙εz − ε˙ θ ) = 0 0 −(αθθ − αzz )η˙ − αθz (˙εz − ε˙ θ ) 0 (9.91) Equation (9.91) is substituted in (9.86) to calculate the plastic spin Wp . On the other hand, the constitutive spin ω is deﬁned in (7.97) as

0 ω = W − Wp = 0 0

0 0 ω

0 −ω 0

(9.92)

where ω = K[(αθθ − αzz )η˙ + αθz (˙εz − ε˙ θ )] − η˙

(9.93)

Since the tensor α is symmetric and the tensor ω is antisymmetric, we have α · ω = −(ω · α)T . Therefore, in order to ﬁnd explicit expressions for the corotational rate, we ﬁrst ﬁnd

0 ω · α − α · ω = 0 0

0 0 −2ωαθz −ω(αzz − αθθ ) 2ωαθz −ω(αzz − αθθ )

(9.94)

Using (9.59), the corotational derivative of α is ∇

α = α˙ − ω · α + α · ω

(9.95)

We then obtain the following expressions by combining (9.95) and (9.83) ∇

α˙ = ω · α − α · ω + α = (ω · α − α · ω) + (µ1 + µ2 )Dp − λα˙z + λα(2) z˙ (9.96) where, from (9.84), α(2) = µ2

z 0

Dp dz z˙

(9.97)

In the last expression, it has been assumed that the corotational axes are parallel to the reference axes, so that M = 1. This is indeed the case for the torsion problems under consideration. The deformation is homogeneous

© 2005 by Chapman & Hall/CRC Press

478

Continuum Mechanics and Plasticity

without rigid-body motion of the tube and the angle of twist per unit length is constant along the tube. In the numerical calculation, we can deﬁne a tensor κ as 0 0 0 κ = ω dt = 0 0 −κ (9.98) 0 κ 0 in which the following expression has been determined by use of (9.93) κ = ω dt = K[(αθθ − αzz )dη + αθz (dεz − dεθ )] − dη

(9.99)

Then, (9.96) reduces to dα = (κ · α − α · κ) + (µ1 + µ2 )Dp dt − λ α dz + λ α(2) dz

(9.100)

The equations derived in this section can be used to describe the response of a thin-walled tube subjected to various combined axial–torsion loading conditions. Two special cases are considered in the following paragraphs. 9.3.3.1 Torsion with axial prestress Denoting the axial prestress by σz = σc = constant, the stress tensor and the deviatoric stress tensor are −σ c 0 0 3 0 0 0 −σc 0 τ and [σ ] = [σ ] = 0 0 τ (9.101) 3 0 τ σc 2σc 0 τ 3 Note that the hoop stress σθ is zero due to symmetry. The ﬂow rule is, from (9.80), (9.89), (9.90), and (9.101), written as σc /3 + αrr dεr =− , dz σy

dεθ σc /3 + αθθ =− dz σy

dεz 2σc /3 − αzz = , dz σy

τ − αθz dη = dz σy

(9.102)

The intrinsic time is then given from (9.79) and (9.89) by ζ˙ 2 = ε˙ r2 + ε˙ θ2 + ε˙ z2 + 2η˙ 2 = z˙ 2 f 2 (z)

(9.103)

Therefore, η˙ 2 =

© 2005 by Chapman & Hall/CRC Press

1 2

z˙ 2 f 2 (z) − ε˙ r2 + ε˙ θ2 + ε˙ z2

(9.104)

Topics in Endochronic Plasticity

479

By use of (9.87), (9.104) reduces to

1 2 2 z˙ f (z) − 2 ε˙ z2 − ε˙ θ ε˙ r 2 1 2 2 dεz 2 dεθ dεr = z˙ f (z) − 2 − 2 dz dz dz

η˙ 2 =

(9.105)

Substituting (9.102) in (9.105), we then obtain 2 2 σ 1 2σ 1 σ c c c ±dη = dz f 2 (z) − − αzz − + αrr + αθθ 2 σy 3 3 3 (9.106) The “+” sign is for loading and “−” is for unloading. To perform the numerical calculation of dα by use of (9.100), α(2) must ﬁrst (2) be determined. To obtain αθz from (9.97), we use (9.89) to get (2)

αθz = µ2

z 0

p

Dθz dz = µ2 z˙

η(z) η(0)

dη = µ2 η

(9.107)

In the last expression, the limits of integration are η(0) = 0 and η(z) = η. Similarly, we obtain the following components for α(2) during loading (2) αrr = µ2 εr ,

(2)

αθθ = µ2 εθ ,

(2) αzz = µ2 εz

(9.108)

Therefore, from (9.98), (9.100), (9.107), and (9.108), we obtain the following equations dαrr = (µ1 + µ2 )dεr − λαrr dz + λµ2 εr dz dαθθ = −2αθz κ + (µ1 + µ2 )dεθ − λαθθ dz + λµ2 εθ dz dαzz = 2αθz κ + (µ1 + µ2 )dεz − λαzz dz + λµ2 εz dz

(9.109)

dαθz = (αθθ − αzz )κ + (µ1 + µ2 )dη − λαθz dz + λµ2 η dz with the initial conditions η(0) = 0, εi (0) = 0, and αij (0) = 0. Thus, in a stepby-step calculation, we can use α = α + dα, εz = εz + dεz ,

εr = εr + dεr , η = η + dη

εθ = εθ + dεθ , (9.110)

Finally, we note that for the case of free-end torsion, the ends of the specimen are totally unconstrained with σc = 0. Thus, the equations for free-end torsion may be obtained by setting σc = 0 in the equations of this subsection.

© 2005 by Chapman & Hall/CRC Press

480

Continuum Mechanics and Plasticity

9.3.3.2 Fixed-end torsion In the case of ﬁxed-end torsion, ε˙ z = 0. Assuming incompressibility, we ﬁnd from (9.87) that ε˙ θ = −˙εr = 0. Hence, (9.89) becomes 0 0 ε˙ r (9.111) [Dp ] = 0 −˙εr η˙ 0 η˙ 0 Note that this is different from the simple shear assumption where ε˙ θ = 0. The stress tensor and the deviatoric stress tensor are −σ 0 0 3 0 0 0 −σ τ [σ ] = 0 0 τ and [σ ] = 0 (9.112) 3 0 τ σ 2σ 0 τ 3 in which σ may vary. Again, we mention that the hoop stress is zero, which is different from the simple shear assumption that σθ = 0. The ﬂow rule, from (9.80), has the following component equations: σ/3 + αrr dεr =− , dz σy αzz

2σ = , 3

σ/3 + αθθ dεθ =− , dz σy

dη τ − αθz = dz σy

(9.113)

The ﬁrst two equations of (9.113) may be combined to yield dεr αθθ − αrr = dz 2σy

(9.114)

The intrinsic time is then, from (9.79) and (9.111), given by ζ˙ 2 = 2˙εr2 + 2η˙ 2 = z˙ 2 f 2 (z) Therefore,

η˙ 2 = z˙ 2

1 2 f (z) − 2

dεr dz

(9.115)

2 (9.116)

Then, by substituting (9.114) in (9.116), we obtain 2 dz αθθ − αrr 2 ±dη = 2f (z) − 2 σy The “+” sign is for loading and “−” is for unloading. © 2005 by Chapman & Hall/CRC Press

(9.117)

Topics in Endochronic Plasticity

481

We may also obtain the following components of α(2) by using the same procedure as that which leads to (9.107) and (9.108) (2)

αθz = µ2 η,

(2) αrr = µ2 ε r ,

(2)

αθθ = −µ2 εr ,

(2) αzz =0

(9.118)

Therefore, from (9.98) to (9.100) and (9.118), we obtain the following component equations dαrr = (µ1 + µ2 )dεr − λαrr dz + λµ2 εr dz dαθθ = −2αθz κ − (µ1 + µ2 )dεr − λαθθ dz − λµ2 εr dz dαzz = 2αθz κ − λαzz dz dαθz = (αθθ − αzz )κ + (µ1 + µ2 )dη − λαθz dz + λµ2 η dz

(9.119)

with the initial conditions η(0) = 0, εr (0) = 0, and αij (0) = 0. We again use (9.110) for a step-by-step calculation.

9.3.3.3 Comparison of theoretical and experimental results In this section, we compare the theoretical and experimental results initially presented in [5] and reprinted here with permission from Elsevier. There are seven material constants in this model: c, β, C1 , σy , µ1 , µ2 , and λ where c and β are used in the isotropic-hardening function f (z) and describe the rate and saturation value of isotropic hardening; C1 ﬁxes the magnitude of plastic spin; σ√ y is a material constant proportional to the initial yield stress in shear (σy = 2τy ); and µ1 , µ2 , and λ are used in the kernel function µ(z), which describes the evolution of back stress. These material constants are determined by ﬁtting the theory to the experimental stress–strain curve during loading. After they have been determined, the constitutive equations are applied to predict experimental results of specimens subjected to different loading conditions. Three different materials have been investigated, 70 : 30 brass, Ni-200, and Al-1100. All shear strains reported in the experimental results are for the outer surface of the tubular specimen. For the 70 : 30 brass material, the material constants have been determined to ﬁt the experimental data of Stout (reported in Im and Atluri [15]) for the case of simple torsion (Figure 9.1). The constants are c = 3.1, β = 15.4, C1 = 4.5, σy = 90 MPa, µ1 = 200 MPa, µ2 = 50 MPa, and λ = 7.2. These constants are then used in the equations for torsion with axial stress σc = 0 (equations in Section 9.3.3.1) to predict behavior of the same material for two different strain paths, that is, monotonic and cyclic free-end torsion. The strain range of the monotonic torsion is from 0 to 4, whereas the specimen under cyclic loading is strained from 0 to 1.7, unstrained back to 0, and then restrained to 2.0. The results found from this theory are compared with the experimental data of Swift [18]. Figure 9.2 shows the axial strain of both monotonic and cyclic free-end torsion. It is seen that the theory does predict the trend of variation for the axial strain during torsion. We note that experiments of Swift and Stout were conducted in different laboratories and material conditions, and © 2005 by Chapman & Hall/CRC Press

482

Continuum Mechanics and Plasticity

Shear stress (MPa)

400

Experiment Theory

300

200

100

0 1

0

2 3 Shear Strain

4

5

FIGURE 9.1 Shear stress–strain curve of 70 : 30 brass (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

12

Monotonic loading Experiment Theory

Shear Stress (%)

10

Cyclic loading Experiment Theory

8 6 4 2 0 –1

0

1

2 Shear Strain

3

4

5

FIGURE 9.2 Axial strain versus shear strain for 70 : 30 brass (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

the agreement demonstrated here is therefore considered as very satisfactory. The effect of C1 is investigated and shown in Figure 9.3 for 70 : 30 brass. This ﬁgure shows the dependence of the axial strain on C1 in the case of monotonic free-end torsion. It is seen that a suitable C1 can be determined to achieve a good agreement with the experimental results.

© 2005 by Chapman & Hall/CRC Press

Axial Strain

Topics in Endochronic Plasticity

483 C1 = 0

35 30 25 20 15 10 5

C1 = 1 C1 = 2 C1 = 5 C1 = 10 C1 = 50 1

2 3 Shear Strain

4

FIGURE 9.3 Effect of parameter C1 of plastic spin on the axial strain during torsion (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

100 90 80

Shear Stress (MPa)

70 60 50 40 30 20 10 0 0

0.2

0.4

0.6

0.8 1 Shear Strain

1.2

1.4

1.6

1.8

FIGURE 9.4 Shear stress–strain curve of Ni-200 with 0.01 MPa axial prestress (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

The experimental data for Ni-200 are taken from Hart and Chang [19]. The material constants have been determined by ﬁtting the shear stress– strain curve (Figure 9.4) which was determined from torsion with a 0.01 MPa prestress. The constants have been determined to be c = 14.2, β = 5.5, C1 = 9, σy = 40 MPa, µ1 = 45 MPa, µ2 = 40 MPa, and λ = 9.5. Using these constants and the constitutive equations of Section 9.3.3.1, we have predicted the axial

© 2005 by Chapman & Hall/CRC Press

484

Continuum Mechanics and Plasticity 0.7 Prestress: Experiment

0.6 0.5

Theory

Axial Strain (%)

0.4

1.48 MPa 0.01 MPa –1.52 MPa

A

A 1.48 MPa B 0.01 MPa C –1.52 MPa B

0.3 0.2 C

0.1 0 –0.1 –0.2 0

0.05

0.1

0.15 0.2 0.25 Shear Strain

0.3

0.35

0.4

FIGURE 9.5 Axial strain for Ni-200 during torsion with axial prestresses (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079, 1995. With permission from Elsevier).

strain associated with torsion with prestresses of 1.48, 0.01, and −1.52 MPa. The results, shown in Figure 9.5, are quite satisfactory. Figure 9.6 shows the experimental shear stress–strain curve under simple shear condition (ﬁxed-end torsion), obtained by White et al. [20] for Al-1100 material. The theoretical result of the present theory is also shown. The material constants are c = 2.14, β = 4.5, C1 = 4.5, σy = 55 MPa, µ1 = 1.8 MPa, µ2 = 0.15 MPa, and λ = 1.64. Wu and Xu [21] also obtained a shear stress– strain curve for Al-1100, but in a smaller deformation range (12% strain). The curve agrees with the one shown in Figure 9.6. Using these constants and the constitutive equations of Section 9.3.3.1, we predicted the axial strain in the case of torsion with prestresses of −6.9 and −20.7 MPa. The results found from this theory (the solid and dashed curves) are compared with the experimental data of Wu and Xu [21] and shown in Figure 9.7. Figure 9.8 shows the prediction (the solid and dashed curves) of the hoop and axial strains, respectively, for the free-end torsion condition (i.e., with σc = 0). The experimental data of Bailey et al. [22] are also shown in the ﬁgure. Even though the theory agrees well with experiment in terms of the axial strain, there are discrepancies in the hoop strain at large shear strain level. These discrepancies may be explained by taking a closer look at the specimens and the procedure used in the experiments of Bailey et al. [22]. The specimens used

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity 250

485

Theory Experiment

Shear stress (MPa)

200

150

100

50

0 0

0.05

0.1

0.15

0.2 0.25 0.3 Shear Strain

0.35

0.4

FIGURE 9.6 Shear stress–strain curve of Al-1100 (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

0

–0.2

Axial Stress (%)

–0.4

–0.6

–0.8

–1

–1.2

Prestress = –6.9 MPa Prestress = –20.7 MPa

–1.4 0

0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09

0.1

Shear Strain FIGURE 9.7 Axial strain for Al-1100 during torsion with compressive axial prestresses (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

486

Continuum Mechanics and Plasticity 10

Axial strain Hoop strain

8 6 4

Strain (%)

2 0 –2 –4 –6 –8 –10 0

1

2

3

4 5 6 Shear Strain

7

8

9

10

FIGURE 9.8 Hoop and axial strains under free-end torsion (From Wu, H.C. et al., Int. J. Solids Struct., 32, 1079,1995. With permission from Elsevier).

by them had a very short gauge length of 3.2 mm (0.125 in.) compared with a radius of 19 mm (0.75 in.). The radius of the relatively rigid ends of the specimen did not change, which in turn restricted the development of hoop strain at large shear strain level. Another possible restriction on the hoop strain is due to a plug and sleeve inserted into the specimens to prevent buckling at large strain level. The authors thought that there was sufﬁcient clearance to allow for any reduction in diameter during test. However, we believe that there was contact between the specimens and the plug at large shear strain level and, therefore, the reduction in diameter was restricted. If there were no contact, then the plug would not have been needed in the experiment. We believe that these are the reasons causing the experimental hoop strain to be on the low side compared with the theoretical result. Wu et al. [23] conducted the same experiments using extruded high purity aluminum with specimens of a much longer gauge length (82.6 mm or 3.25 in.) and without the plug. The outer radius of the specimens was 19 mm (0.75 in.). The results are shown in Figure 9.9. It is seen that these curves have the same trends as those of the theoretical curves shown in Figure 9.8, that is, the hoop and axial strains at large shear strain level have almost the same magnitude, whereas the results of Bailey et al. [22] show that the hoop strain does not increase much with the axial strain at large shear strain level. In some published writings such as Canova et al. [24], the rate of hoop strain is assumed to be equal to the rate of radial strain, ε˙ θ = ε˙ r , for a thin-walled

© 2005 by Chapman & Hall/CRC Press

Axial and Hoop Strain (%)

Topics in Endochronic Plasticity

487

6 al S Axi

4 2

–2 –4

train

Shear Strain (%) 25

50

75 100 125 150 175 Hoo p Str ain

–6

FIGURE 9.9 Experimental hoop and axial strains under free-end torsion (From Wu, H.C. et al, Int. J. Plasticity, 13, 873, 1998. With permission from Elsevier).

tube under tension–torsion loading condition. This assumption is good only for the axial loading condition. Taylor and Quinney [25] showed that the hoop strain is not equal to the radial strain under combined tension–torsion loading. In this calculation, we have found that the rate of radial strain is almost zero, that is, the wall thickness changes very little. And, from (9.87), the magnitude of the hoop strain is nearly the same as that of the axial strain, in agreement with the experimental observation. We mention that the analysis of Lowe and Lipkin [26] and Qian and Wu [27], by use of polycrystal plasticity, also leads to the same trends as predicted by our theory for the axial and hoop strains.

9.4

An Endochronic Theory for Porous and Granular Materials

Porous-granular (PG) material is a class of material that includes geotechnical materials (concretes, rocks, soils, ice, etc.), porous metals made out of metal powders by sintering, and ceramics. The response of PG materials to loading generally consists of four parts, that is, the hydrostatic response, the deviatoric response, the shear-enhanced volumetric response, and the hydrostatic pressureenhanced shear response. A signiﬁcant characteristic of this class of materials is the existence of voids (or cracks) within the material. The pores collapse and close or grow under loading–unloading conditions, and material is either consolidated or damaged. This process is irreversible (plastic deformation and damage) and upon removal of the load a permanent change in the volume of the specimen is observed. Thus, plastic volumetric strain occurs when PG materials are subjected to hydrostatic pressure. Figure 9.10 shows a schematic volumetric stress–strain curve with both the initial and the ﬁnal slopes equal to the elastic bulk modulus K0 . The deviatoric stress–strain response for this class of materials is similar to that observed for metallic materials. A phenomenon similar to yielding occurs as the deviatoric stress–strain curve bends toward the strain axis.

© 2005 by Chapman & Hall/CRC Press

Continuum Mechanics and Plasticity

Hydrostatic Stress

488

Volumetric Strain FIGURE 9.10 Schematic volumetric stress–strain curve for porous-granular materials (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

0 < th

Volumetric Strain

0

Shear Strain

0 < th 0

Shear Strain 0 > th

0

Shear Strain

FIGURE 9.11 Shear-enhanced volumetric strain (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

A special property of PG materials is that during the application of deviatoric stress, a specimen exhibits a volumetric change that can either be a contraction or dilation depending on the state of hydrostatic stress σ 0 as compared with a threshold stress σ th within the specimen. This coupled behavior between volumetric and deviatoric responses is generally referred to as the shear-enhanced volumetric strain or densiﬁcation in soil mechanics. Figure 9.11 illustrates this behavior. Another coupled behavior is the hydrostatic pressure-enhanced shear deformation, which is sometimes referred to as the shear travel. In the last effect, additional deviatoric deformation occurs as the hydrostatic stress increases, while keeping the deviatoric stress constant. Figure 9.12 shows that along stress-paths BC, DE, and FG, on which the deviatoric stress is kept constant, shear travel occurs as is seen by the increase

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

489 G G F

Hydrostatic Stress

E

C

F

E

D z

C

B

D

Hydrostatic Axis

A A O

B

O

2x,y

Deviatoric Strain

FIGURE 9.12 The shear travel effect (From Wu, H.C. and Aboutorabi, M.R., Int. J. Plasticity, 4, 163, 1988. With permission from Elsevier).

in the deviatoric strain for each of the path segment. A threshold deviatoric stress may be deﬁned above which the shear travel strain is positive and below which it is negative. The hydrostatic and deviatoric responses may be viewed as the primary behavior while the coupled responses are secondary. In a theoretical treatment, the degree of importance of each response is therefore different. The hydrostatic and deviatoric responses should be the main part of a constitutive equation and they are directly related to both yield surface and ﬂow rule if such concepts are used in the formulation. However, there may indeed be cases in which no such concepts are used. In such cases, the hydrostatic and deviatoric responses should still be the main part of a constitutive equation. The coupled effects are secondary and can be accounted for by the ﬂow rule or by the evolution equation of a parameter. They also inﬂuence the shape of yield surfaces. In the case of soils, the most common test for the study of their mechanical behavior has traditionally been the conventional constant conﬁning pressure triaxial test (simply known as the conventional triaxial compression, CTC). In such a test, a cylindrical specimen is prepared in a ﬂexible membrane of a material such as polyurethane, and is placed in a chamber that can be pressurized, usually by ﬁlling it with water. An all-around constant conﬁning pressure is applied. Then, a loading ram can be used to apply an axial load along the long axis of the cylinder. In this test, the mean stress increases with the axial load and the observed stress–strain behavior is a combination of hydrostatic–deviatoric behavior. This test is denoted by CTC in Figure 9.13 and the stress path for this test is making an angle with HC (the hydrostatic compression). The stresses in this ﬁgure are principal stresses. σz is the axial stress of the cylindrical specimen. Unconﬁned compression tests (UC) and conﬁned compression tests (CC) have been used to test materials such as concretes, rocks, and ice. Cylindrical specimens are tested in the axial

© 2005 by Chapman & Hall/CRC Press

490

Continuum Mechanics and Plasticity z TC

UC

CTC

HC

CC TE 2 x,y

FIGURE 9.13 Illustration of various tests in the stress space.

direction either with free lateral surface (UC) or conﬁnement in a rigid cell (CC). The lateral stress builds up with increasing axial stress in the CC test. Both tests involve the mean stress and the deviatoric stress. The aforementioned traditional tests are not designed to separate the hydrostatic behavior from the deviatoric behavior. Since both behaviors are of primary importance in the characterization of PG materials, the true triaxial test has been developed to test the hydrostatic and deviatoric behaviors separately. The true triaxial device permits application of three independent (principal) stresses on a cubical specimen. The application of the stresses can be such that any path of loading in the three-dimensional stress space can be followed. Some of the paths are shown in Figure 9.13. The HC path corresponds to the application of an all-around hydrostatic pressure in isotropic consolidation. TC stands for triaxial compression and TE stands for triaxial extension. In the latter two tests, the deviatoric stress is applied under the condition of constant hydrostatic pressure, enabling us to concentrate on the deviatoric stress–strain response. Finally, we mention that direct shear testing and torsion of a solid shaft have also been conducted by researchers to characterize material behavior in shear. In this section, a version of endochronic theory of plasticity is presented that accounts for all the aforementioned responses. This theory has been derived based on the work of Wu and Aboutorabi [28] and Wu [29]. It is presented here with permission from Elsevier. We present the theory ﬁrst and its applications to concretes, sand, and porous aluminum are discussed.

9.4.1

The Endochronic Equations

The theory as derived in [28] has four elements corresponding to those previously mentioned. It has been modiﬁed in [29] so that the strain-rate sensitivity may be accounted for. The stress–strain curve is decomposed into volumetric and deviatoric stress–strain curves. The decomposition gives insight into

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

491

material behavior and is of special importance due to the signiﬁcant role played by the plastic volumetric deformation. This theory uses the Gibbs formulation described in Section 8.3.4. The Gibbs free energy is a function of stress σ and two groups of internal variables, γ and π. There are h number of γ’s related to the volumetric deformation and s number of π’s related to the deviatoric deformation. The reason for using the Gibbs formulation is that the hydrostatic and deviatoric stresses may be independently varied, which is a requirement for the derivation of the set of equations to be discussed in this chapter. This requirement is difﬁcult to satisfy in the Helmholtz formulation, since in that case the strain, ε is used as an independent variable and it is difﬁcult to independently vary the volumetric and the deviatoric strains for the PG materials. A hydrostatic intrinsic time zH is deﬁned to register the history of volumetric deformation, and a deviatoric intrinsic time zD is used to register the history of deviatoric deformation. In the Gibbs formulation, strain εij is given by εij = −

∂ ∂σij

(9.120)

and the evolution equations for γijh and πijs are given by h dγkm =0 dzH

(h not summed)

s dπkm ∂ s + N =0 ijkm ∂πijs dzD

(s not summed)

∂ ∂γijh

h + Mijkm

(9.121)

h and M s are positive semideﬁnite fourth-order isotropic constant where Mijkl ijkl tensors. These linear evolution equations are chosen for mathematical simplicity and they can be nonlinear if. However, they are shown to be adequate for the class of materials under consideration. These evolution equations are related to the rate of entropy production within the material. By expanding the Gibbs free energy in series and using only the quadratic and linear terms, the expression for may be substituted into (9.120) to (9.121). Each resulting equation can then be divided into volumetric and deviatoric parts. By doing so, it may be found that the volumetric strain εkk is the sum of the H , and densiﬁcation strain, ε S . The deviatoric strain e is hydrostatic strain, εkk ij kk the sum of strain due to deviatoric loading, eijS , and strain developed due to the coupling with the hydrostatic loading, eijH . The internal variables are divided into two parts as h γijh = 13 δij γkk + gijh ,

© 2005 by Chapman & Hall/CRC Press

s πijs = 13 δij πkk + pijs

(9.122)

492

Continuum Mechanics and Plasticity

where gijh is the deviatoric part of γijh , pijs is the deviatoric part of πijs , and δij is the Kronecker delta. The intrinsic times ζH and ζD are deﬁned by dζH = kH θ˙kk |dθkk |

and

˙ 2 dQij dQij dζD2 = kD (Q)

(9.123)

where the volumetric strain-like increment dθkk is deﬁned as H dθkk = dεkk − k1

dσkk 3K0

(9.124)

and the deviatoric strain-like tensor dQij is deﬁned as dQij =

deijS

− k2

dσij

(9.125)

2µ0

where σ = σkk /3 = mean pressure, σij = deviatoric stress; k1 and k2 are constants between 0 and 1. In the limiting case that k1 = k2 = 1, θkk reduces to the usual deﬁnition of volumetric plastic strain and Qij reduces to the deviatoric plastic strain. K0 is the bulk modulus and µ0 is the shear modulus. ˙ are the strain-rate sensitivity functions (see The functions kH (θ˙kk ) and kD (Q) Section 8.4.6), which enable the description of the strain-rate sensitive stress– strain behavior in the volumetric and deviatoric responses, respectively. 1/2 . ˙ ˙ ˙ where Q ˙ = (1Q These are functions of the strain-rates θ˙kk and Q, 2 ij Qij F) The following expressions may be used

θ˙kk kH (θ˙kk ) = 1 − kh log ˙θkk0

,

˙ = 1 − kd log kD (Q)

˙ Q ˙ Q0

(9.126)

˙ 0 are reference strain rates usually where kh and kd are constants; θ˙kk0 and Q taken as the lowest strain rates of the test series. Then, the following deﬁnes the governing equations for each component of strain: Volumetric: H = 3A0 σkk + 3 εkk

h Bh0 γkk

h

dγ h M0h kk dzH

h + Eh0 γkk − Bh0 σkk = 0

dζH = h(ζH ) dzH

© 2005 by Chapman & Hall/CRC Press

for all h (no sum on h)

(9.127)

Topics in Endochronic Plasticity

493

Deviatoric: eijS = A2 σij +

C2s pijs

s

dpijs N2s dzD

+ F2s pijs − C2s σij = 0

for all s (no sum on s)

(9.128)

dζD = f (ζD , σ 0 ) dzD Shear-enhanced volumetric strain: S = εkk

s s s C0 πkk

dπ s

s − Cs (σ − ξ ) = 0, N0s dzkk + F0s πkk 0 kk D

dπ s

s − Cs σ = 0, N0s dzkk + F0s πkk 0 kk D

s=1

(9.129)

s = 1

Pressure-enhanced shear strain: eijH =

h h h B2 gij

dgh

M2h dz ij + Eh2 gijh − Bh2 (σij − Dij ) = 0, H

dgh

M2h dz ij + Eh2 gijh − Bh2 σij = 0, H

h=1

(9.130)

h = 1

In the above equations, f (ζD , σ 0 ) = the deviatoric-hardening function, σ 0 = conﬁning hydrostatic stress at initial shear loading, A0 , A2 , Bh0 , Bh2 , C0s , C2s , Eh0 , Eh2 , F0s , F2s , M0h , M2h , N0s , N2s = parameters of the theory (for engineering application, they can be combined and the number of material constants reduced), ξ = threshold mean conﬁning pressure, Dij = threshold deviatoric stress. The equations for hydrostatic and deviatoric responses are now further investigated. These equations can be written in a form such that, in the limiting case of k1 = k2 = 1, yield conditions can exist with respect to both the hydrostatic and deviatoric stresses. This case also enables a geometric representation of the model in the stress space, so that the physical meaning of the model may be visualized. The geometric representation is further explained. The values of k1 and k2 do not have to be one. A value of 0.95 has been found to facilitate numerical computation. In this case, the constitutive equations are continuous and there is the advantage of not having to deal with the yield conditions in the numerical calculation. This aspect is indeed a very important strength of the present approach. In this way, even though yield stress is deﬁned in the theory, it can be circumvented during computation by assuming k1 not equal to one. In this approach, the results will be closely related to

© 2005 by Chapman & Hall/CRC Press

494

Continuum Mechanics and Plasticity

those obtained from the case of k1 = k2 = 1, where the yield conditions are used. The equations for hydrostatic and deviatoric responses are considered further in the following subsections.

9.4.1.1 The hydrostatic response H and the linear evolution for internal The volumetric strain increment dεkk h are from (9.127) given by variable γkk H = 3A0 dσkk + 3 dεkk

h dγkk Bh Eh h = 0h σkk − 0h γkk dzH M0 M0

h Bh0 dγkk ,

h

(9.131)

In order to account for strain hardening, the intrinsic time zH is scaled by dζH = h(θkk , ζH ) dzH

(9.132)

where the function h represents isotropic hardening and the increment of volumetric intrinsic time dζH > 0 is deﬁned in terms of plastic strain as in (9.123). The form of the hardening function is h(θkk ) =

C − (C − θm )e−µθkk θm − θkk

(9.133)

This form accounts for the experimentally observed fact that as material compacts, its ability to undergo plastic volumetric strains diminishes and eventually an elastic response is observed with a modulus equal to the initial bulk modulus. Thus, a maximum plastic volumetric strain of θm may be achieved. The material constants C and µ control the extent and rate of isotropic hardening. The values of these constants may be adjusted to ﬁt the volumetric stress–strain curves of various PG materials, including soil. By the substitution of (9.123), (9.124), (9.132), and the second equation of (9.131) into the ﬁrst equation of (9.131), the following equations may be found H dεkk [1 ± X] =

dσkk [1 ± k1 X] 3K0

(9.134)

where X=

Xh

h

© 2005 by Chapman & Hall/CRC Press

with X h =

Bh0 hM0h

h = Bh0 σkk − Eh0 γkk

(9.135)

Topics in Endochronic Plasticity

495

h = 0. Hence, the constant A may be Note that k1 = 1 and initially σkk = γkk 0 identiﬁed, that is, A0 = 1/9K0 and when h → ∞, (9.134) yields

dσkk 1 · 3 K0

H = dεkk

(9.136)

Equation (9.136) indicates a linear stress–strain response with a slope equal to the initial bulk modulus at large volumetric strain. When loading reverts to unloading the only change in the equations takes place in (9.134), where the negative sign in the brackets changes to positive. Note that in this investigaH and the current tion, tensile stress is considered to be positive. Knowing dεkk h values of zH , σkk and γkk , (9.134) may be used to calculate dσkk . (9.123), (9.124), and (9.132) can then be used to determine dθkk and dzH , and (9.131) leads to h . Therefore, z , σ , and γ h can be updated. This step-by-step procedure dγkk H kk kk is used to calculate the volumetric stress–strain curve. For the case of k1 = 1, it is shown now that the previous equations can describe a physical situation when the material experiences a combined isotropic–kinematic hardening in the volumetric behavior. Both tensile (further limited by fracture) and compressive hydrostatic stresses are included in this discussion and it is shown that the combined isotropic–kinematic hardening arises naturally in the volumetric response of the endochronic formulation. To this end, the ﬁrst equation of (9.131) is solved for dσkk and the result substituted into (9.124) to obtain H + 3k1 dθkk = (1 − k1 )dεkk

Bh Bh 0 0

h

=

H ϕkk

M0h

σkk −

Bh Eh 0 0

h

M0h

h dzH γkk

H + ψkk dzH

(9.137)

where H H = (1 − k1 )dεkk ϕkk Bh Bh Bh E h H 0 0 0 0 h ψkk = 3k1 σ − γ h kk h kk M M 0 0 h h

(9.138)

But, from (9.123) and (9.132), H H h dzH = dζH = ±kH dθkk = ±kH (ϕkk + ψkk dzH )

(9.139)

or H ∓ βkk

© 2005 by Chapman & Hall/CRC Press

h kH

H dzH + ϕkk =0

(9.140)

496

Continuum Mechanics and Plasticity

H = 0. Thus, When k1 = 1, ϕkk

H ψkk ∓

h kH

dzH = 0

(9.141)

Since during plastic deformation, dzH = 0, then, H =± ψkk

h kH

(9.142)

By substituting (9.138) into (9.142), it is found that y

H σkk − αkk

σ = ± kk h kH

(9.143)

where y σkk

= 3

Bh Bh

−1

0 0 M0h

h

y

H αkk = 3σkk

and

Bh Eh 0 0

h

M0h

h γkk

(9.144)

This expression may be viewed as a yield criterion for hydrostatic stress with y H denoting the kinematic σkk h/kH denoting the isotropic hardening and αkk y hardening. Note that in the isotropic hardening, σkk is the initial quasistatic yield stress, which when divided by kH becomes the dynamic yield stress. h is the isotropic-hardening function. The ﬂow rule is given from (9.137) by dzH

H dzH = dθkk = ψkk

9.4.1.2

y

σkk

H (σkk − αkk )

(9.145)

The deviatoric response

In the deviatoric response, from (9.128), the equations are deijS

=

A2 dσij

+

dpijs

C2s dpijs ,

dzD

s

=

C2s F2s s σ − p N2s ij N2s ij

(9.146)

Note that the evolution of pijs is deﬁned with respect to the deviatoric intrinsic time zD . For the ﬁrst increment of loading from the virgin state, since σij = pijs = 0, (9.146) yields

deijS dσij

© 2005 by Chapman & Hall/CRC Press

= A2 0

(9.147)

Topics in Endochronic Plasticity

497

Therefore, A2 is identiﬁed as the inverse of the initial slope 2µ0 of the deviatoric stress–strain curve. Thus, A2 = 21 µ0 . The deviatoric intrinsic time increment dζD is deﬁned as in (9.123) and is related to zD through the hardening function f (zD ) deﬁned by (9.128). It will be shown subsequently that function f represents isotropic hardening in the deviatoric behavior. Solving the ﬁrst equation of (9.146) for dσij and substituting the result together with the second equation of (9.146) into (9.125) yields dQij = ϕijD + ψijD dzD

(9.148)

ϕijD = (1 − k2 )deijS Cs F2s s 2 ψijD = k2 C2s σ − p N2s ij N2s ij s

(9.149)

where

Then, by substituting the third equation of (9.128) and (9.148) into (9.123), the following quadratic equation is obtained 2 P dzD + W dzD + R = 0

(9.150)

where P = ψijD ψijD −

f kD

2 ,

W = 2ϕijD ψijD ,

R = ϕijD ϕijD

(9.151)

Therefore, P, W , and R are functions that are deﬁned in terms of the constants of the model and increments of input variables. When (9.150) is solved for dzD , the second equation of (9.146) can be used to obtain dpijs . By substitution, the deviatoric stress increment dσij can then be found from the ﬁrst equation of (9.146). In the case of k2 = 1, (9.149) and (9.151) give ϕijD = R = W = 0. Thus, (9.150) 2 = 0. Since dz = 0 when there is plastic deformation, is reduced to P dzD D P must be zero. Hence, the ﬁrst equation of (9.151) leads to (σij

− αijD )(σij

− αijD )

=

σy f

2 (9.152)

kD

where σy

=

Cs Cs s

© 2005 by Chapman & Hall/CRC Press

2 2 N2s

−1 ,

αijD = σy

Cs F s

2 2 s pij

s

N2s

(9.153)

498

Continuum Mechanics and Plasticity

This is the Mises yield criterion with combined isotropic–kinematic hardening, in which σy f /kD describes the isotropic hardening and αijD the kinematic hardening in the deviatoric behavior. Note that in the isotropic hardening, σy is the quasistatic deviatoric yield stress, which when divided by kD becomes the dynamic yield stress and f is the isotropic-hardening function. From (9.148), the plastic strain increment is now given by p

deij = ψijD dzD =

dzD σij − αijD σy

(9.154)

which is normal to the deviatoric yield surface. It has thus been shown that in the case of k1 = k2 = 1, the present endochronic theory is equivalent to a ﬂow theory of plasticity, which obeys the Mises yield criterion with combined isotropic–kinematic hardening, both in the hydrostatic and deviatoric responses. 9.4.1.3 Geometric representation of the model There is a simple geometrical representation of the proposed model for the case of k1 = k2 = 1, in which two yield criteria are deﬁned, one for volumetric behavior and the other for deviatoric behavior. The material constants of the model depend on the initial density of the material, and these constants are then used to describe subsequent material behavior. The two yield criteria exist in a space plotting the hydrostatic stress σkk /3 against the equivalent stress σeq , which is deﬁned as the square root of the second invariant of the deviatoric stress tensor (see Figure 9.14). The volumetric yield criterion is represented by two vertical yield lines and the deviatoric yield criterion by two horizontal yield lines. These yield lines are not necessarily straight due to the cross effects between the hydrostatic and deviatoric responses. These are shown by the thin curves in Figure 9.14. The distance eq Vol. Elastic Line

Vol. Yield Line

Deviatoric Yield Line 0

Vol. Yield Line

kk/3

Deviatoric Yield Line

FIGURE 9.14 Geometric representation of the model (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

499

between the yield lines can expand, resulting in isotropic hardening. The two yield lines as a set can also move, resembling the kinematic hardening. According to this model, combined isotropic–kinematic hardening takes place in both the volumetric and deviatoric responses. A volumetric elastic line may be established in the hydrostatic compression region indicating a limit beyond which the volumetric response is elastic again. This phenomenon corresponds with the bending upward of the volumetric stress–strain curve at large strain level, where the modulus is elastic. According to this model, the volumetric and deviatoric yield limits are individually imposed. The model allows for the situation that yielding has already occurred volumetrically but not yet occurred deviatorically. This is a situation that is frequently observed in sands, which have a very low volumetric yield limit. Thus, the deviatoric response in this case would initially be elastic and then plastic when the deviatoric yield limit is reached. In the case of sand, the volumetric yield lines are collapsed into a line passing through the origin as shown in Figure 9.15. In this ﬁgure, compressive stress is considered positive as is the usual practice of soil mechanics. The failure lines (FL) are shown together with lines showing the initial yield lines and the subsequent yield lines obtained by isotropic and kinematic hardening, respectively. The idea of volumetric compaction yield surface and shear yield surface and ! of representing them as horizontal and vertical straight lines in the J1 versus J2 space was brieﬂy mentioned by Johnson and Green [30]. This idea is similar to the present model and is described by the endochronic constitutive equations of this section.

eq FL

Subsequent YL Deviatoric initial YL

kk/3

0

Volumetric YL

Kinematic hardening Initial YL Isotropic hardening FL

FIGURE 9.15 Yield lines for sand (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

© 2005 by Chapman & Hall/CRC Press

500

Continuum Mechanics and Plasticity deijh

eq

dQij

dQij

TC

s dkk

dkk

s dkk

CT or C PL

Deviatoric YL

dkk

0

HC

kk/3

Volumetric YL

FIGURE 9.16 Plastic strain increments of the model (From Wu, H.C., in Modern Approaches to Plasticity, Elsevier, Amsterdam, 1993. With permission from D. Kolymbas).

The volumetric plastic strain increment dθkk is given by (9.145) and the deviatoric plastic strain increment dQij is given by (9.154), which is normal to the deviatoric yield surface. These equations resemble the ﬂow rule of a ﬂow theory of plasticity. However, additional plastic strain increments S and deH need to be considered in this model. These increments are due dεkk ij to coupled effects as discussed earlier and the occurrence of the increments depends on the stress path. Figure 9.16 shows the plastic strain increments associated with various stress paths in a true triaxial test. A hydrostatic compression test (HC) will give rise to dθkk only; a TC test will give rise to dQij S ; and a CTC test or a proportional loading test (PL) will lead to all and dεkk S , and deH . It is difﬁcult to compare the four increments, that is, dθkk , dQij , dεkk ij present plastic strain increments with the associative or nonassociative ﬂow rules of the classical theory. In that theory, the direction of the total plastic strain increment is investigated with respect to a plastic potential in the stress space, and combines both the deviatoric and hydrostatic behaviors. Whether the ﬂow rule is associative or nonassociative is still a point of debate. In the present model, no such complication is involved, however.

9.4.2

Application to Concrete

The endochronic theory of the previous section has been applied in [28] to investigate the experimental results of concrete reported by Scavuzzo et al. [31]. Cubical specimens were tested under a true triaxial test. In such a test, σx , σy , σz are principal stresses and εx , εy , εz are principal strains.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

501

The material is not strain-rate sensitive and the strain-rate sensitivity functions are kH = kD = 1. For the isotropic-hardening functions, (9.133) is used for h and the form for f is chosen as f (zD ) = Cp − (Cp − 1)e−µzD

(9.155)

where Cp and µ are constants. Equations of Sections 9.4.1.1 and 9.4.1.2 are used to describe the hydrostatic and deviatoric behaviors. In the consideration of shear-enhanced volumetric strain, we use two internal variables, and (9.129) becomes S 1 2 εkk = C01 πkk + C02 πkk 1 dπkk C1 = 0 (σkk − ξ ), dzD N

2 dπkk C2 F2 2 = 0 σkk − 0 πkk dzD N N

(9.156)

All deviatoric constants associated with the internal variable π 1 are assumed to be zero. The above equations may be combined to yield S dεkk S = I 1 (σkk − ξ ) − χ 2 εkk + I1χ 2 dzD

zD 0

(σkk − ξ ) dzD + I 2 σkk + χ 2 π0 (9.157)

where I1 =

C01 C01 , N

I2 =

C02 C02 , N

χ2 =

F02 , N

1 2 π0 = C01 πkk (0) = −C02 πkk (0)

(9.158) Following Wu et al. [32], ξ = σth . In addition, I 1 , I 2 , χ 2 , and π0 may be determined to complete the characterization of the shear-enhanced volumetric strain response. Finally, we mention that the shear travel effect is determined by use of (9.130). In an effort to describe the experimental data for concrete obtained by Scavuzzo et al. [31], the endochronic equations presented for the hydrostatic, deviatoric, shear-enhanced volumetric strain, and pressure-enhanced shear strain were solved by Wu and Aboutorabi [28] in an iterative incremental fashion utilizing a computer. The increment in stress path is input into a program that computes from it an increment for the hydrostatic stress and one for the deviatoric stress. Then, accordingly, the hydrostatic and deviatoric modules are called on to ﬁnd the corresponding increment of strains and increment of intrinsic time. If any coupling strains are to be evaluated, then the increments of the intrinsic times are passed on to the shear-enhanced volumetric strain and pressure-enhanced shear strain modules to ﬁnd such strains. Any

© 2005 by Chapman & Hall/CRC Press

502

Continuum Mechanics and Plasticity 100 Principal Stress (MPa)

(a)

Theory Experiment si

4k

1

50

= 1 si 8k

=

3

2

2,3 0 0

100 Principal Stress (MPa)

(b)

2

4 6 8 10 Principal Strain (*1000)

12

Theory Experiment

50

1 4

0 –5

0 4. .5 2 .5 = 3 1 2 = 1 8 6

2,3

0 5 10 Principal Strain (*1000)

15

FIGURE 9.17 Behavior of concrete subjected to various stress paths — inserts show stress paths (From Wu, H.C. and Aboutorabi, M.R., Int. J. Plasticity, 4, 163, 1988. With permission from Elsevier).

stress path that is neither purely hydrostatic nor deviatoric is approximated by a staircase path (i.e., as a series of consecutive hydrostatic and deviatoric increments). The outputs of the theoretical computations are presented in [28]. They constitute a rather extensive study of various stress paths. It is fair to say that the model has done a good job in describing such a diverse loading program. In Figure 9.17(a) and (b), we show two cases. For each stress path the stress–strain relations in both 1- (vertical) and 2-directions are presented. The 1-direction is marked with ◦ and the 2-direction with . Since the tests are all performed in the deviatoric plane, the loadings in the 2- and 3-directions are the same and the result for the 3-direction is identical to that for the 2-direction.

9.4.3

Application to Sand

Sand is a cohesionless soil. It has mechanical properties similar to those described in the introductory paragraphs of Section 9.4. They are the hydrostatic response, the deviatoric response, the shear-enhanced volumetric response, and the hydrostatic pressure-enhanced shear response. In the

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

503

terminology of soil mechanics, the hydrostatic response is known as isotropic consolidation. The volumetric stress–strain curve bends toward the stress axis. The deviatoric behavior depends on hydrostatic stress (or the normal stress) and the deviatoric (or shear) stress–strain curve bends toward the strain axis. There is no shear strength at zero conﬁning pressure. The shear-enhanced volumetric response is also known as densiﬁcation or dilation. The ﬁrst application of the endochronic theory to the description of mechanical behavior of sand was due to Bazant and Krizek [33], using the simple endochronic theory (see Section 8.4.2). Valanis and his coworkers [34,35] have also contributed extensively to this subject. Our approach is different from aforementioned works in that we use the Gibbs formulation. The equations are similar to those presented in Section 9.4.1. Using this formulation, Wu and Wang [36] obtained theoretical results of isotropic consolidation and deviatoric response, which compare favorably with experimental results of Lade [37] for Sacramento River sand subjected to loading–unloading. In addition, the shear hysteretic loops for loose crystal silica No. 20 sand reported in [38] were theoretically investigated in [36]. We [36] also investigated densiﬁcation and the results compared favorably with those reported in [39]. The shear hysteresis of sand was further investigated by Wu and Sheu [40] using a method of integration similar to that discussed in Section 8.4.5.2, resulting in closed-form solutions. The theory predicted the test results of Silver and Seed [41] at the 1st, 2nd, 10th, and 300th cycles reasonably well. Nine cases of relative densities and vertical stresses were considered. Additional works in the endochronic modeling of sand are Wu et al. [32] considering a true triaxial test and Wu and Aboutorabi [42] considering sand behavior subjected to a circular stress path. Furthermore, the undrained response of sand was discussed in [29].

9.4.4

Application to Porous Aluminum

Recent developments in the techniques of powder metallurgy (P/M) have made it possible to solidify all kinds of metallic powders into structure components of controlled porosity. Application of endochronic theory to describe the phenomenological behavior of porous aluminum was carried out by Aboutorabi et al. [43], and Wang and Wu [44]. However, these applications were limited to isotropic consolidation and monotonic uniaxial straining, using the experimental results of Schock et al. [45] and some limited experimental data for high-purity aluminum P/M. Using specimens of high-purity aluminum P/M, Wu et al. [46] conducted a series of experiments under various cyclic straining conditions and showed that the endochronic theory presented in Section 9.4.1 can be used to describe the experimental results reasonably well. The theory of Section 9.4.1 has four elements. They are the hydrostatic response, the deviatoric response, the densiﬁcation, and the shear travel. Although densiﬁcation and shear travel are two important coupled behaviors

© 2005 by Chapman & Hall/CRC Press

504

Continuum Mechanics and Plasticity

between hydrostatic and deviatoric elements, their determination cannot be accomplished by uniaxial stress experiments and awaits further investigation by use of other specimen conﬁgurations and loading conditions. In [46], these two effects are neglected, and the efforts have been focused on the evaluation of the hydrostatic and deviatoric behaviors subjected to cyclic loading. Due to consistent results obtained even with this approximation, it may be concluded that densiﬁcation and shear travel are of secondary importance for the material tested under uniaxial stress condition. The decomposition of the axial stress–strain curve into volumetric and deviatoric stress–strain curves gives further insight into the material behavior. This is of special importance due to the signiﬁcant role played by the plastic volumetric deformation. The hydrostatic and deviatoric elements of the endochronic theory are now discussed separately and concepts of the present formulation are interpreted in terms of those of the classical plasticity. In a uniaxial strain-controlled test, the strain and stress states are ε1 0 0 σ1 0 0 [ε] = 0 ε2 0 , (9.159) [σ ] = 0 0 0 0 0 0 0 0 ε2 where 1 is in the axial direction of the cylindrical specimen. The volumetric strain is εv = ε1 + 2ε2 and the mean stress is σkk = σ1 /3. The deviatoric strain and stress are 2 0 0 3 (ε1 − ε2 ) , [e] = 0 − 13 (ε1 − ε2 ) 0 1 0 0 − 3 (ε1 − ε2 ) (9.160) 2 0 0 3 σ1 [σ ] = − 31 σ1 0 1 0 − 3 σ1 The hydrostatic response is described by (9.133) and (9.134). Several cyclic straining paths were tested. One of them is shown in Figure 9.18(a) and another in Figure 9.18(b). Both theoretical and experimental results are shown in the ﬁgures. Only one internal variable p is used for simplicity in the discus = −2σ = −2σ and e = sion of the deviatoric response. Since we have σ11 11 22 33 −2e22 = −2e33 , only the 11-components of (9.146) and (9.125) are independent equations. Combing these equations and (9.123) with kD = 1, we obtain de11 [1 ± XD ] =

dσ11 [1 ± k2 XD ] 2G0

(9.161)

where " XD =

© 2005 by Chapman & Hall/CRC Press

3 C2 (C2 σ11 − F2 p11 ) 2 f N2

(9.162)

Topics in Endochronic Plasticity

505

30

(a)

Theory Experiment

Hydrostatic Stress (MPa)

20 10 0 –10 –20 –30 –0.15

–0.05

0.05

0.15

0.25

Volumetric Strain (%) (b)

25

Theory Experiment

20 Hydrostatic Stress (MPa)

15 10 5 0 –5 –10 –15 –20 –25 0.00

0.05

0.10

0.15

0.20

0.25

Volumetric Strain (%) FIGURE 9.18 Cyclic volumetric stress–strain curve for porous aluminum: (a) test program 1, (b) test program 2 (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

The hardening function is f (zD ) = CD − (CD − 1) exp(−µzD )

(9.163)

Equations (9.161) and (9.163) are used in a numerical procedure to compute the deviatoric stress–strain curves. Figures 9.19(a) and (b) are the deviatoric counterparts of Figures 9.18(a) and (b).

© 2005 by Chapman & Hall/CRC Press

506

Continuum Mechanics and Plasticity 50

Deviatoric Stress (MPa)

(a)

Theory Experiment

25

0

–25

–50 –1 –0.8 –0.6 –0.4 –0.2 0

0.2 0.4 0.6 0.8

1

Deviatoric Strain (%) 50

Deviatoric Stress (MPa)

(b)

Theory Experiment

25

0

–25

–50 0

0.2

0.4

0.6

0.8

1

Deviatoric Strain (%)

FIGURE 9.19 Deviatoric counterparts of Figure 9.18 (From Wu, H.C. et al., Int. J. Plasticity, 6, 207, 1990. With permission from Elsevier).

9.5 9.5.1

An Endochronic Formulation of a Plastically Deformed Damaged Continuum Introduction

Typical work in continuum damage mechanics (CDM) often involves the damage-effect variables in the sense of Kachanov [47] and the effective stress/effective strain concepts. Consequently, damage mechanics theories are often derived from the usual constitutive theories by use of effective variables, which take into account the effects of damage, in place of

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

507

original variables. The thermodynamics framework of CDM often involves the concept of either the strain equivalence postulate [48] or the strain-energy equivalence postulate [49,50], or the hypothesis of stress working equivalence [51] along with the concepts of continuum mechanics and irreversible changes in the material internal structure. The microdefects are represented at the macroscopic level by a damage variable. A typical elastoplastic damage theory is based on the generalized damage theory initially proposed by Chaboche [52] and later by Lemaitre [53]. In [53], Lemaitre proposed that the damage energy release rate, that is, energy release by the system during the damaging process, is related to the elastic strain energy. The damage energy release rate is deﬁned by the thermodynamic force conjugate to damage evolution. This treatment amounts to an uncoupled consideration between plasticity and damage processes. These concepts of CDM have been proposed by different authors associated with different deﬁnitions and theories, and not all of them are needed in one theory. Some of the aforementioned concepts and deﬁnitions are not even compatible with each other. Following the work of Wu and Nanakorn [54], we discuss the existing concepts of CDM and propose a CDM constitutive framework using a set of concepts in a uniﬁed manner. The reproduction of [54] is with permission from Elsevier. Further constitutive modeling is required to arrive at explicit constitutive equations for CDM, which may be achieved by use of a concept such as damage potential within the proposed constitutive framework. Another approach is to formulate the constitutive equations based on an endochronic concept and still using the same constitutive framework. The endochronic formulation for CDM is discussed in this section.

9.5.2

The Anisotropic Damage Tensor

This work uses a second-order tensor as a parameter of damage. The tensor deﬁnes the loss of net area of material as in the original work of Kachanov [47]. The presentation of damage tensor Dij in this section follows previous work by Murakami and Ohno [55] and Betten [56], in which the damage tensor is constructed using area vectors related to Cauchy’s tetrahedron in a damaged state. In Murakami and Ohno’s anisotropic damage theory of creep, the second-rank symmetric damage tensor Dij is derived by representing the effects of microscopic grain-boundary cavities in terms of a dyadic product of the unit normal vector to the relevant boundary. On the other hand, in a macroscopic approach, Betten derived the damage tensor from a third-order, skew-symmetric, continuity tensor that represents the area vector. In [54], the derivation of Dij is similar to Betten’s derivation, but a second-order continuity tensor is used, which provides a simple and more meaningful physical interpretation. Consider a differential tetrahedron of an undamaged material as shown in Figure 9.20(a). Note that the ﬁgure shows a special case where xi axes coincide (j) with the principal damage axes. In general, if dSi denotes the i-component of

© 2005 by Chapman & Hall/CRC Press

508

Continuum Mechanics and Plasticity x3

(a)

(b)

x3

(4) dSi

dx3

– (4)

dSi = dSi(4)

dx3

(1)

– (1)

dSi

dSi x2

(2)

x2

– (2)

dx2

dSi

dSi

dx1

dx2 dx1

x1

(3) dSi

– (3) (3) dSi = dSi

x3

(c)

(4)

(4)

dSi = ij dSi

dx3 (1)

dSi

x2 (2) dSi

dx2 dx1

x1

– (3)

(3)

dSi = dSi

FIGURE 9.20 Deﬁnition of damage measure-load bearing area: (a) undamaged continuum, (b) actual damaged continuum, (c) ﬁctitious undamaged continuum (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

(j)

(j)

a gross area element that has the normal nk , then dSi can be characterized by (1)

= − 12 eijk dxj dxk

(2)

= − 12 eijk dxj dxk

(3)

= − 12 eijk dxj dxk

(4)

= − 12 eijk (dxj

dSi dSi dSi

(2)

(3)

(3)

(1)

(1)

(2)

(1)

dSi

(9.164) (3)

(2)

(3)

− dxj )(dxk − dxk ) (j)

where eijk is the permutation tensor and the vectors dxi do not coincide with the principal damage axes in the general case. The sum of these vectors is zero due to closure of the surface area of tetrahedron, that is (1)

dSi

© 2005 by Chapman & Hall/CRC Press

(2)

+ dSi

(3)

+ dSi

(4)

+ dSi

= 0i

(9.165)

Topics in Endochronic Plasticity

509

Consider now a tetrahedron of a material with internal damage as shown in Figure 9.20(b). The nominal dimensions of this tetrahedron are the same as those for Figure 9.20(a), but the areas are reduced by scalar factors α, β, γ , and κ from the previous tetrahedron with their corresponding normals unchanged. Then, the area vectors are (1)

= − 12 αijk dxj dxk = α dSi

(2)

= − 12 βijk dxj dxk = β dSi

(3)

= − 12 γijk dxj dxk = γ dSi

(4)

= − 12 κijk (dxj

dS¯ i dS¯ i dS¯ i dS¯ i

(2)

(3)

(1)

(3)

(1)

(2)

(1)

(2)

(3)

(1)

(3)

(9.166)

(2)

(3)

(4)

− dxj )(dxk − dxk ) = κ dSi

where αijk = αeijk , βijk = βeijk , γijk = γ eijk , and κijk = κeijk . The areas in (9.166) represent net cross-sectional areas of the element. These are the areas that are effectively resisting loads and are perpendicular to the coordinate (4) axes x1 , x2 , and x3 , respectively. Note that dS¯ i denotes the inclined side. The parameters α, β, and γ are discussed further later in this section. We (1) (4) note that the vectors dS¯ i , . . . , dS¯ i , deﬁned in (9.166), and the correspond(1) (4) ing dSi , . . . , dSi deﬁned in (9.164), differ in length, and the condition of closure cannot be satisﬁed, that is (1)

dS¯ i

(2)

+ dS¯ i

(3)

+ dS¯ i

(4)

+ dS¯ i

= 0i

(9.167)

except for the case of isotropic damage where α = β = γ = κ. Because of the existence of microcavities in the material, the load-carrying net areas of the damaged continuum, Figure 9.20(b), are reduced. It is now postulated that there exists a ﬁctitious undamaged continuum, as shown in Figure 9.20(c), which is mechanically equivalent to the damaged continuum. Thus, the damage state is represented by the ﬁctitious undamaged continuum such that (1)

= − 12 eijk dˆxj dˆxj

(2)

= − 12 eijk dˆxj dˆxj

(3)

= − 12 eijk dˆxj dˆxj

(4)

= − 12 eijk (dˆxj

dSˆ i dSˆ i dSˆ i dSˆ i

© 2005 by Chapman & Hall/CRC Press

(2)

(3)

(1) = dS¯ i

(3)

(1)

(2) = dS¯ i

(1)

(2)

= dS¯ i

(1)

(9.168)

(3)

(3)

(2)

(3)

− dˆxj )(dˆxk − dˆxk )

510

Continuum Mechanics and Plasticity (j)

where dˆxi deﬁne the ﬁctitious differential tetrahedron. Furthermore, the closure of the ﬁctitious undamaged continuum is assumed to be satisﬁed. Thus, (1)

dSˆ i

(2)

+ dSˆ i

(3)

+ dSˆ i

(4)

+ dSˆ i

= 0i

(9.169)

(j) (j) The three area vectors dSˆ i in (9.168) are identical to the vectors dS¯ i (j) in (9.166) and are related to the vectors dSi in (9.164) by scalar factors (4) (4) α, β, and γ , respectively. The fourth vectors dSˆ i and dS¯ i are different in both magnitude and direction. Since (9.168) is used in the remaining part of this chapter, the parameter κ is not important and is not discussed further. (4) (4) It is reasonable to assume that dSˆ i and dSi are related by a linear relation (4)

dSˆ i

(4)

= ψij dSj

(9.170)

(4) where ψij is a second-order tensor. In (9.170), dSˆ i represents the effective (4) load-carrying area of the damaged material and dSj is the gross area on the inclined face of the material element. Therefore, tensor ψij represents the (4) fraction of dSj that can be used to carry load, accounting for the effect of damage. Tensor ψij is known as the continuity tensor, since it describes the continuity state of the material. The continuity tensor ψij can be determined directly from (9.170). Substituting (9.164) and (9.165) into the right-hand side of (9.170), and (9.166), (9.168), and (9.169) into the left-hand side of (9.170), we obtain (2)

(3)

(3)

(1)

(1)

(2)

αijk dxj dxk + βijk dxj dxk + γijk dxj dxk (2)

(3)

(3)

(1)

(1)

(2)

= ψir erjk (dxj dxk + dxj dxk + dxj dxk )

(9.171)

(j)

If the vectors dxi are aligned with the coordinate axes xi , respectively, then (j)

dxi

= δij |ds j | (no sum on j), where |ds j | deﬁnes the magnitude of the (j)

vector dxi . Then, for i = 1, (9.171) becomes (ψ11 − α)e123 |ds2 ||ds3 | + ψ12 e231 |ds3 ||ds1 | + ψ13 e321 |ds1 ||ds2 | = 0 (9.172) (j)

Since |ds j |, the magnitudes of dxi , are independent of each other, they can be independently varied. But, due to the closure assumption, (9.172) cannot be violated. Therefore, (9.172) can be satisﬁed for all values of |ds j |, if and only if ψ11 = α,

© 2005 by Chapman & Hall/CRC Press

ψ12 = 0,

ψ13 = 0

(9.173)

Topics in Endochronic Plasticity

511

Similar discussions may be used for i = 2 and 3. Thus, the continuity tensor is found to be α 0 0 (9.174) [ψ] = 0 β 0 0 0 γ It is seen that when the xi axes are principal damage axes, the continuity tensor ψij is in a diagonal form. In the case of uniaxial tension along the x1 direction, let s be the total gross cross-sectional area and sˆ be the effective area of resistance so that sˆ < s. (4) (4) In view of (9.170), vectors dSˆ i and dSi are represented by [ˆs, 0, 0]T (4) and [s, 0, 0]T , respectively, with ni = [1, 0, 0]T . Then, by use of (9.174), (9.170) reduces to sˆ = ψs

(9.175)

where ψ = ψ11 = α. Therefore, ψ = sˆ/s represents that fraction of the crosssectional area which can be used to resist load. When ψ = 1, the material is in the virgin state without damage and sˆ is identical to s. When ψ = 0, the material can no longer resist load, since its effective area of resistance is reduced to zero. The damage tensor is deﬁned as a complementary (dual) tensor of continuity [57]. In other words, the damage tensor represents the fraction of the cross-sectional area that was reduced by microdefects. In the uniaxial loading case, the damage variable can be expressed in terms of the continuity variable ψ as D=

s − sˆ =1−ψ s

(9.176)

Thus, D = 0 corresponds to the undamaged state and D = 1 corresponds to the breaking state of the material. In the multiaxial case, a second-order damage tensor Dij is deﬁned as Dij = δij − ψij

(9.177)

Note that Dij is the damage tensor and is not to be confused with the rate of deformation tensor used in most chapters of this book. In the special case, when the xi axes are also the principal axes of damage, tensor ψij is given by (9.174), and the damage tensor is given by

D1 [D] = 0 0

© 2005 by Chapman & Hall/CRC Press

0 D2 0

0 1−α 0= 0 0 D3

0 1−β 0

0 0 1−γ

(9.178)

512

Continuum Mechanics and Plasticity

It is seen that the principal values D1 , D2 , and D3 are related to the principal continuity variables α, β, and γ , respectively. These principal values Di can be measured on the test specimens cut along mutually perpendicular directions x1 , x2 , and x3 , respectively. Alternatively, the continuity tensor is given in terms of the principal values of the damage tensor as

α [ψ] = 0 0

0 β 0

0 1 − D1 0 = 0 γ 0

0 1 − D2 0

0 0 1 − D3

(9.179)

where α = 1 − D1 , β = 1 − D2 , and γ = 1 − D3 .

9.5.3

Gross Stress, Net Stress, and Effective Stress

In the previous section, a deﬁnition of damage is derived by introducing a ﬁctitious undamaged continuum that is mechanically equivalent to the actual damaged continuum. In this section, various deﬁnitions of stress, such as the gross stress, the net stress, and the effective stress, are discussed. The gross stress or the Cauchy stress, σij , is the stress deﬁned on the actual damaged continuum while the net stress, σˆ ij , and the effective stress, σ˜ ij , are the nonsymmetric and symmetric stress, respectively, deﬁned on the ﬁctitious undamaged continuum. By considering the actual damaged continuum and the ﬁctitious undamaged continuum under the same applied force, the corresponding stresses on the two continua are different, since the stresses are calculated over different cross-sectional areas of the continua. If the equilibrium of the actual damaged continuum is considered (Figure 9.21(a)), one can derive the relation between the stress vector ti and the stress tensor σij , that is, ti = σji nj

(9.180)

where ni is the unit normal of an area element dS. Similarly, the equilibrium of the ﬁctitious undamaged continuum, with an area element dSˆ and unit normal nˆ i (Figure 9.21(b)) yields tˆi = σˆ ji nˆ j

(9.181)

where σˆ ij is the net stress acting on the ﬁctitious undamaged continuum and tˆi is the corresponding stress vector. Since the area elements dS and dSˆ are subjected to the same force, that is, dPˆ i = dPi , we can conclude that dPi = ti dS = σji nj dS = σˆ ki nˆ k dSˆ = tˆi dSˆ = dPˆ i

© 2005 by Chapman & Hall/CRC Press

(9.182)

Topics in Endochronic Plasticity x3

(a)

513 (b)

dPi

dx3

x3

dPi = dPi

dx3

ni

21

ni

21 x2

x2

dx2

22 23

dx2

22

dx1

23

x1

(c)

x3

dx1

x1

~ dPi

dx3

~ n n i = i

21 x2 dx2

22

23

dx1

x1

FIGURE 9.21 Deﬁnitions of stress tensor and pseudo-force: (a) Cauchy stress, (b) net stress, (c) effective stress (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

where dS and dSˆ are scalar quantities and the corresponding vector expression is obtained from (9.170) as nˆ i dSˆ = ψij nj dS. Thus, (9.182) becomes (σji − σˆ ki ψkj )nj dS = 0

(9.183)

and it follows that σij = ψki σˆ kj

and

σˆ ij = ψik−1 σkj

(9.184)

By use of (9.174), the net-stress σˆ ij is found to be σ

11

α σ21 [σˆ ] = β σ31 γ

σ12 α σ22 β σ32 γ

σ13 α σ23 β σ33

(9.185)

γ

which shows that the net-stress σˆ ij is nonsymmetric, except for the case of isotropic damage. It is not convenient to use the nonsymmetric stress

© 2005 by Chapman & Hall/CRC Press

514

Continuum Mechanics and Plasticity

tensor σˆ ij together with a symmetric strain tensor and strain rate in the constitutive equations. Therefore, new symmetric stress measures, the effective stress σ˜ ij , have been deﬁned on the ﬁctitious undamaged continuum and used in the constitutive equations. Various deﬁnitions have been proposed to symmetrize σˆ ij . These deﬁnitions may be summarized based on various transformations operated on the net stress σˆ ij . They are 1. Betten [56] proposed a transformed net-stress tensor, which is an effective stress subjected to the following transformation σ˜ ij = 12 (σˆ ij ψkj−1 + ψki−1 σˆ jk )

(9.186)

Using (9.184), the expression becomes −1 σ˜ ij = 12 (ψik−1 ψij−1 + ψjk−1 ψmi )σkm = Mijkm σkm

(9.187)

where −1 Mijkm = 12 (ψik−1 ψij−1 + ψjk−1 ψmi )

(9.188)

The fourth-order transformation tensor Mijkm is referred to as the damage-effect tensor. For ψij to have the diagonalized form of (9.174), (9.187) is expressed in the matrix form as

1 α2 σ˜ 11 σ˜ 22 σ˜ 33 = σ˜ 12 σ˜ 23 σ˜ 31

0 1 β2

0

0

0

0

0

0

1 γ2

0

0

1 αβ

0

sym

1 βγ

0 0 σ11 σ22 0 σ33 σ12 0 σ23 σ31 0 1 γα

(9.189)

or σ11 α2

σ12 [σ˜ ] = αβ σ 13 αγ which is a symmetric tensor.

© 2005 by Chapman & Hall/CRC Press

σ12 αβ σ22 β2 σ23 βγ

σ13 αγ σ23 βγ σ33 γ2

(9.190)

Topics in Endochronic Plasticity

515

2. The effective stress proposed by Cordebois and Sidoroff [58], also by Chow and Wang [59], is deﬁned through its components given by σ˜ ij =

# σˆ ij σˆ ji

(no sum on i or j)

(9.191)

Since the right-hand side of (9.191) is not a tensor operation, the effective stress σ˜ ij as deﬁned by (9.191) is not a tensor. However, in the matrix form, the above deﬁnition of effective stress can also give rise to a linear relationship between σ˜ ij and σij . 3. In a study of anisotropic damage in ductile solids, Stumvoll and Swobada [60] deﬁned the effective stress as the symmetric part of the net-stress tensor, that is, −1 σ˜ ij = 12 (σ˜ ij + σ˜ ji ) = 12 (ψik−1 δjm + δik ψjm )σkm

(9.192)

where the damage-effect tensor is −1 ) Mijkm = 12 (ψik−1 δjm + δik ψjm

(9.193)

By use of (9.179), Mijkm may be written in terms of the principal damage D1 , D2 , and D3 and it can be reduced to a form used by Rabotnov [61] and later by Chow and Lu [62]. In all cases, the effective stress σ˜ ij is related to the Cauchy stress σij by the equation σ˜ ij = Mijkm σkm

(9.194)

where the exact expression for the damage-effect tensor Mijkm depends on the method used in symmetrizing σˆ ij . With respect to the principal damage coordinate system, the damage-effect tensor Mijkm is represented by a 6 × 6 diagonal matrix. In a special case, if the directions of principal stresses coincide with those of the principal damage, then these equations further reduce to σ˜ 11 0 0 M1111 σ11 σ˜ 22 = 0 M2222 0 σ22 (9.195) σ˜ 33 σ33 0 0 M3333 where M1111 , M2222 , and M3333 are functions of principal damage variables D1 , D2 , and D3 . The interpretation of the effective stress is now investigated. The net-stress tensor σˆ ij is an actual nonsymmetric stress acting on the ﬁctitious, undamaged continuum, which is subjected to the same applied force as the original, actual,

© 2005 by Chapman & Hall/CRC Press

516

Continuum Mechanics and Plasticity

damaged continuum, that is, dPˆ i = dPi . On the other hand, the effective stress tensor σ˜ ij is the ﬁctitious symmetric stress acting on the ﬁctitious undamaged continuum due to the application of the pseudo-force dP˜ i , as shown in Figure 9.21(c). To validate this statement, the Cauchy formula, relating the pseudo-force dP˜ i to the effective stress σ˜ ij is dP˜ i = σ˜ ji nˆ dSˆ

(9.196)

where nˆ i and dSˆ were previously deﬁned on the ﬁctitious undamaged element. Using (9.170) and (9.194), the above relation can be rewritten in terms of the Cauchy stress and the area element ni dS as dP˜ i = Mjikm σkm nˆ j dSˆ = Mjikm σkm ψjr nr dS

(9.197)

If Betten’s deﬁnition of the damage-effect tensor (9.188) is used, (9.197) becomes dP˜ i = ψij−1 dPj

(9.198)

This equation establishes that the pseudo-force dP˜ i is related to the original applied force dPi by the inverse-transpose of the continuity tensor ψij . If, on the other hand, the damage-effect tensor is deﬁned by (9.193), then the pseudo-force on the ﬁctitious undamaged element is ˆ = 1 (dPi + ψ −1 σjk nˆ j dS) ˆ dP˜ i = 12 (dPi + σˆ ij nˆ j dS) 2 ik

(9.199)

ˆ due to the nonsymmetric property We note that dPi = σˆ ji nˆ j dSˆ = σˆ ij nˆ j dS, of σˆ ij . The last term of (9.199) can be viewed as an additional abstract-force due to the actual stress σij acting over the area of the ﬁctitious undamaged ˆ Therefore, the pseudo-force corresponding to this continuum, that is, nˆ j dS. deﬁnition of effective stress has no simple physical interpretation. 9.5.4

An Internal State Variables Theory

Based upon concepts of continuum mechanics and irreversible thermodynamics with internal variables, the Clausius–Duhem inequality (with thermal gradient) with respect to the actual, damaged continuum is given by (see [63]) ˙ ij , qrij , Dij , γijs , θ) − ηθ˙ − σij ε˙ ij − (ε

1 hj θ,j ≥ 0 θ

(9.200)

In (9.200), the Helmholtz free energy is a function of total (elastoplastic) strain εij , damage measure Dij , temperature θ, and two sets of internal

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

517

state variables qrij and γijs . There are n number of internal variables qrij (r = 1, 2, . . . , n), which describe the state of plastic deformation, and m number of internal variables γijs (s = 1, 2, . . . , m), which specify the state of damage in the continuum. hi is heat ﬂux vector and η is entropy density. In a typical damage mechanics model, the damage tensor Dij is treated as an internal state variable (it is macroscopically not measurable by deﬁnition) that describes the irreversible process of internal structure due to microdefects. However, in the present work, the damage tensor Dij is not an internal state variable and it represents a measurable quantity, that is, the fraction of reduction in load-resisting area. It is a measurable quantity in the description of damage, even though it may be difﬁcult to measure. The role played by Dij in the description of damage is similar to the role played by strain, which is also measurable, in the description of plastic deformation. In [54], a set of internal state variables γijs has been introduced to describe the state of internal damage as a result of growth and/or nucleation of microcracks and/or microvoids. The set of m internal variables γijs , which evolves with loading histories, is introduced to distinguish one internal state of damage from the others, similar to the set of internal variables qrij which describes the state of plastic deformation that cannot be uniquely described by the plastic strain alone. The damage variable Dij describes the current fraction of area reduction but not the state of damage. To elaborate, two continua of the same initial damaged state, when undergoing different loading histories, may end up having the same load-resisting area momentarily, hence the same value of Dij , but having two different states of damage. The concept of using both damage tensor Dij and damage internal state variables γijs in [54] is similar but not equal to the concept of Krajcinovic [64] proposed for the brittle CDM model. In Krajcinovic’s model, the microcracks vector ﬁelds ω(i) , treated as internal variables, are used to describe the state of damage, and a scalar damage measure D is used to describe the overall damage of the material. However, D is the macroscopic counterpart of the microscopic ω(i) (they are related by an integral) and D is, therefore, not measurable. In the present work, Dij is deﬁned by a deﬁnition not directly related to γijs and it is inﬂuenced by the current loading condition. Thus, at the same state of damage, a different incremental loading state will give rise to a different increment of Dij . Hence, dDij is different when the material element is subjected to incremental tension, compression, or shear. As an illustration, consider uniaxial tension of a cylinder. The majority of the microcracks will develop in the plane perpendicular to the maximum tensile strain. If the specimen is then unloaded and subsequently subjected to a small compressive stress along its axial direction, the specimen will behave as though it were undamaged up to a certain compressive stress threshold, since all of the microcracks will be passive (crack closure). Consequently, the initial increment of Dij depends on whether the stress increment is tensile or compressive, even though the state of damage is the same at that moment. Furthermore, with the second-order tensor representations of Dij and γijs , the theory [54] is capable of describing both spherical (e.g., void volume fraction) and

© 2005 by Chapman & Hall/CRC Press

518

Continuum Mechanics and Plasticity

planar (e.g., a system of planar microcracks) effects of microcracks, and their interactions. In the ﬁctitious undamaged conﬁguration, the volume and surface area of the continuum are reduced by excluding the volume and area of the continuum that were previously occupied by microdefects. These are denoted by ˆ and S, ˆ respectively. Consequently, the ﬁctitious undamaged matrix material V becomes homogeneous and isotropic. For a given force ﬁeld Pˆ i = Pi , the ﬁrst law of thermodynamics written for this ﬁctitious undamaged continuum is 1 d ˆ ˆ ˆ ˆ ˆ ˆ ρˆ bi vˆ i dV + (σˆ ji vˆ i − hj )nˆ j dS + rˆ dV vˆ i vˆ i + εˆ ρˆ dV = dt Vˆ 2 ˆ ˆ V Sˆ V (9.201) where ( ∧ ) is used to indicate that the quantity is associated with the ﬁctitious undamaged continuum. In (9.201), vˆ i is the velocity; εˆ is the internal energy density; ρˆ is the mass density; bˆ i is the body force; and rˆ is the heat source term. The ﬁrst term in the surface integral represents the rate of work done by surface traction and is expressed in terms of the nonsymmetric netstress tensor σˆ ij . When the pseudo-force ﬁeld P˜ i is introduced to the ﬁctitious continuum so that the corresponding effective stress σ˜ ij is symmetric, (9.201) is written as d 1 ˆ ˆ ˆ ˆ = ˆ ˆ ˜ ˜ ˜vi v˜ i + εˆ ρˆ dV ˆ rˆ dV ρˆ bi vi dV + (σ˜ ji vi − hj )nj dS + dt Vˆ 2 ˆ ˆ V Sˆ V (9.202) Due to the use of pseudo-force ﬁeld P˜ i , the velocity vector in this conﬁguration is v˜ i instead of vˆ i , as indicated in (9.202). Consequently, the deformation of the ﬁctitious undamaged continuum subjected to pseudo-force ﬁeld P˜ i is different from that subjected to force ﬁeld Pi . The rate of deformation for the ﬁctitious undamaged conﬁguration is then deﬁned by ∂ v˜ ˙ε˜ ij = 1 ∂ v˜ i + j (9.203) 2 ∂xj ∂xi where ε˜ ij deﬁnes the deformation of the ﬁctitious undamaged continuum (with pseudo-force ﬁeld P˜ i ) and is referred to as the effective strain. According to (9.203), the relationship between the effective strain ε˜ ij and the actual strain εij depends on transformations between velocity vectors from vi to vˆ i and from vˆ i to v˜ i . In general, the explicit forms of these transformations are difﬁcult to deﬁne due to the complexity of the geometry and mathematics involved. In this work, the effective strain ε˜ ij is expressed in terms of damage tensor Dij and actual strain εij , and this relationship is discussed later in this section. The postulate of free energy equivalence is applied in the subsequent discussion. According to this postulate, which was initially proposed

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

519

by Cordebois and Sidoroff [58] in the form of strain-energy equivalence, the free energy for an actual, damaged material has the same form as that for a ﬁctitious, undamaged material, but the variables are replaced by the effective quantities. Thus, ˜ ε˜ ij , q˜ rij , γijs , θ ≡ εij , qrij , Dij , γijs , θ (9.204) where the q˜ rij ’s are the effective qrij ’s. Note that Dij does not explicitly appear as one of the state variables on the left-hand side of (9.204). In view of (9.204), the free energy available to do mechanical work and stored in the ﬁctitious continuum is the same as that stored in the actual continuum, resulting in an equivalent mechanical behavior. The second law of thermodynamics and the equation of motion at the ﬁctitious conﬁguration subjected to the pseudo-force ﬁeld P˜ i become d dt

ˆ V

ˆ ≥ ρη ˆ dV

ˆ V

rˆ ˆ dV − θ

ˆ hi nˆ j dSˆ Sˆ θ

∂ σ˜ ji + ρˆ bˆ i = ρˆ f˜i ∂xi

(9.205) (9.206)

where fˆi = d˜vi /dt. Using (9.202) to (9.206), the Clausius–Duhem inequality for the ﬁctitious undamaged continuum in the isothermal condition is given by ˙˜ ε˜ , q˜ r , γ s ≥ 0 σ˜ ij ε˙˜ ij − (9.207) ij ij ij so that

˜ ∂ σ˜ ij − ∂ ε˜ ij

˜ ˜ s ∂ ∂ ε˙˜ ij − r q˙˜ rij − γ˙ ≥ 0 ∂ q˜ ij ∂γijs ij

(9.208)

In the ﬁctitious continuum, ε˜ ij , q˜ rij , and γijs are the state variables so that they can be independently varied. Although, q˜ rij may vary when ε˜ ij changes, their relation is not one-to-one. Different ε˜ ij histories may lead to the same q˜ rij , and a material with different q˜ rij may correspond to the same ε˜ ij momentarily. Thus, it is possible to vary ε˜ ij so that q˜ rij is left unchanged. Therefore, inequality (9.208) is always satisﬁed, if σ˜ ij =

˜ ∂ ∂ ε˜ ij

and

−

˜ r ˜ s ∂ ∂ γ˙ ≥ 0 q˙˜ ij − r ∂ q˜ ij ∂γijs ij

(9.209)

According to the ﬁrst equation of (9.209), the effective stress σ˜ ij is derivable ˜ The inequality (9.209) gives the from the ﬁctitious undamaged free-energy . thermodynamic constraints on the laws governing the evolution of the two sets of internal variables, q˜ rij and γijs .

© 2005 by Chapman & Hall/CRC Press

520

Continuum Mechanics and Plasticity

It is now possible to derive the explicit relationship for effective strain ε˜ ij . A relation similar to the ﬁrst equation of (9.209) exists for the actual damaged continuum. When the postulate of free energy equivalence is assumed, this relation is σij =

˜ ˜ ∂ ε˜ mn ˜ ∂ q˜ rmn ∂ ∂ ∂ ∂ = = + r ∂εij ∂εij ∂ ε˜ mn ∂εij ∂ q˜ mn ∂εij

(9.210)

where the effective internal variable q˜ rij is assumed to be a function of the actual internal variable qrij and damage tensor Dij . Note that, for the actual damaged continuum s independent variables are εij , qrij , and Dij , so that the second term on the right-hand side of (9.210) drops out and the equation reduces to σij =

˜ ∂ ε˜ mn ∂ ε˜ mn ∂ = σ˜ mn ∂ ε˜ mn ∂εij ∂εij

(9.211)

Using (9.194), (9.211) further reduces to ∂ ε˜ mn = Nijmn ∂εij

(9.212)

where Nijmn is the inverse of Mijmn and is a function of Dij only, or Mijmn Nrsij = Imnrs

(9.213)

In (9.213), the fourth-order identity tensor is Iijkm = δik δjm and δij is Kronecker’s delta. Thus, it follows from (9.212) that the effective strain ε˜ ij is linearly related to εij by ε˜ ij = Nkmij εkm

or

εij = Mkmij ε˜ km

(9.214)

Then, it is assumed that the following relations are valid for the internal variable qrij q˜ rij = Nkmij qrkm

or

qrij = Mkmij q˜ rkm

(9.215)

Constitutive equations at the ﬁctitious undamaged conﬁguration must satisfy the inequality given by (9.207). By use of (9.214) this inequality can be written as ˙˜ ε , q˜ r , γ s ) + σ˜ ∂ ε˜ km D ˙ ij ≥ 0 σij ε˙ ij − (˜ ij ij ij km ∂Dij

(9.216)

∂ ε˜ ij ∂Nrsij = εrs ∂Dmn ∂Dmn

(9.217)

where

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

521

By observing (9.204), the ﬁrst two terms of (9.216) are the same as the lefthand side of (9.200) in the isothermal case. During an incremental loading, the ﬁctitious undamaged continuum undergoes a deformation in the matrix as well as an increase in damage. The ﬁrst two terms of (9.216) are energy dissipated associated with this process. However, by deﬁnition, the state of the ﬁctitious material remains undamaged at the end of each loading increment. The amount of energy dissipated in order to restore the ﬁctitious continuum to the undamaged state is represented by the last term of inequality (9.216). For convenience, inequality (9.216) can be rewritten as ˙˜ ε˜ , q˜ r , γ s − G D ˙ σij ε˙ ij − ij ij ij ij ij ≥ 0

(9.218)

where Gij = −σ˜ km

∂ ε˜ km ∂Dij

(9.219)

Tensor Gij is the thermodynamic force associated with unit damage growth ˙ ij , and, in this work, it is referred to as the “damage force” for simplicity. This D quantity may also be considered as the energy release rate per unit damage advance. Physically, the negative of the damage force, −Gij , can be interpreted as the “restoring force” that restores the ﬁctitious continuum to its undamaged ˙ ij . It is seen from (9.219) that state after experiencing a unit damage growth D Gij can be expressed in terms of σ˜ ij , ε˜ ij , and Dij . A further discussion of the damage force can be found in the appendix of [54].

9.5.5

Plasticity and Damage

We now characterize the plastic deformation process, the damage process, and the coupling between the two processes. Starting with the actual damaged conﬁguration, where the state variables are εij , Dij , qrij , and γijs , the Clausius– Duhem inequality (9.200) can be rewritten for isothermal process as σij ε˙ ij −

∂ ∂ ∂ ˙ ∂ s Dij − ε˙ ij − r q˙ rij − γ˙ ≥ 0 ∂εij ∂qij ∂Dij ∂γijs ij

(9.220)

˜ and noting that Dij and γ s are independent variables, (9.220) Replacing by ij becomes ˜ ∂ ε˜ ij ˜ ∂ q˜ rij r ˜ ∂ ε˜ ij ˜ ∂ q˜ rij ∂ ∂ ∂ ∂ ˙ km σij ε˙ ij − D ε˙ km − r r q˙ km − + r ∂ ε˜ ij ∂εkm ∂ q˜ ij ∂qkm ∂ ε˜ ij ∂Dkm ∂ q˜ ij ∂Dkm −

˜ s ∂ γ˙ ≥ 0 ∂γijs ij

© 2005 by Chapman & Hall/CRC Press

(9.221)

522

Continuum Mechanics and Plasticity

or, after regrouping of terms, it may be shown that ˙˜ ε˜ , q˜ r , γ s ≥ 0 σij ε˙ ij − ij ij ij

(9.222)

Constraint (9.222) represents the Clausius–Duhem inequality of the actual damaged conﬁguration. However, unlike (9.200), inequality (9.222) involves ˜ εij , q˜ r , γ s ), which is deﬁned in the ﬁctithe ﬁctitious free energy (˜ ij ij tious undamaged conﬁguration, where the ﬁctitious material is isotropic. ˜ εij , q˜ r , γ s ) involves only material constants that are isotropic Therefore, (˜ ij ij tensors. In an attempt to characterize the plastic deformation and the damage process, one recognizes that the damage process does not directly inﬂuence the mechanisms of plastic deformation; that is, there is no direct coupling between damage and plastic deformation. In general, plasticity is directly related to slips for metals and to other mechanisms for other materials. In all cases, damage inﬂuences plastic strains only because the net area of resistance decreases as the damage proceeds. In the present work, damage does not directly inﬂuence plastic deformation of the ﬁctitious undamaged continuum, but it does inﬂuence the plastic deformation of the actual continuum. Based on this ˜ εij , q˜ r , γ s ) is assumed to consist of observation, the ﬁctitious free energy (˜ ij ij ˜ 1 (˜εij , q˜ r ) and the damage potential two parts, the ﬁctitious plastic potential ij ˜ 2 (Dij , γ s ), that is, ij

˜ ε˜ ij , q˜ rij , γijs = ˜ 1 ε˜ ij , q˜ rij + ˜ 2 Dij , γijs

(9.223)

˜ 1 (˜εij , q˜ r ) characterizes the plastic process of the ﬁctitious where potential ij ˜ 2 (Dij , γ s ) describes the damage undamaged continuum while potential ij process. During deformation, the microcracks and microvoids will extend, grow, and nucleate, resulting in progressive material deterioration. This damage deterioration is not arbitrary and it must obey thermodynamic ˜ 2 (Dij , γ s ) is used to constraints to be established. The damage potential ij provide the equation of damage evolution and its necessary constraints. The state of microdefects is represented by the set of internal variables γijs . The change in microdefects together with the loading condition bring about a decrease in load-resisting area, which is represented at the macroscopic level by damage tensor Dij . The effect is carried over to the deformation process, elastic or plastic, through the effective variables, σ˜ ij , ε˜ ij , and q˜ rij . Hence, an indirect coupling occurs between the plasticity and damage in the actual damaged continuum. Using (9.223), inequality (9.222) is written as ˙˜ D , γ s ≥ 0 ˙˜ ε˜ , q˜ r − σij ε˙ ij − ij ij 1 ij ij 2

© 2005 by Chapman & Hall/CRC Press

(9.224)

Topics in Endochronic Plasticity 9.5.6

523

The Constitutive Equations and Constraints

Within an inﬁnitesimal strain theory, the stress rate is usually represented by the material rate. In CDM, it is important, however, to consider the rotation of the principal directions of damage during the deformation process. The principal directions of damage do not generally coincide with the principal stress, when nonproportional loading takes place or when the material has suffered a prior damage. To satisfy the requirements of reference frame indifference, the rate of change of damage measure Dij and the internal variables γijs are expressed by the corotational derivatives ˙ D∇ ij = Dij − ωik Dkj + Dik ωkj ,

γijs∇ = γ˙ijs − ωik γkjs + γiks ωkj

(9.225)

where ωij represents the spin of the principal damage coordinate frame with respect to the ﬁxed reference coordinate frame. Thus, it follows from (9.224) that ˜ 1 ∂ ε˜ km ˜ 1 ∂ q˜ rkm r ∂ ∂ σij − ε˙ ij − r q˙ ∂ ε˜ km ∂εij ∂ q˜ km ∂qrij ij ˜ 1 ∂ q˜ rkm ˜2 ˜ s∇ ˜ 1 ∂ ε˜ km ∂ ∂ ∂ ∂ D∇ + r + γ ≥0 (9.226) − ij − ∂ ε˜ km ∂Dij ∂ q˜ km ∂Dij ∂Dij ∂γijs ij Since εij , Dij , qrij , and γijs are independent state variables, ﬁxing these values ˜ 1 , and ˜ 2 because they are state functions. For also ﬁx the values of σij , inequality (9.226) not to be violated for any arbitrary choice of ε˙ ij while keeping Dij , qrij , and γijs unchanged, the following conditions must hold σij =

˜ 1 ∂ ε˜ km ∂ , ∂ ε˜ km ∂εij ˜ 1 ∂ q˜ rkm r ∂ − r q˙ − ∂ q˜ km ∂qrij ij

(9.227a)

˜ 1 ∂ ε˜ km ˜ 1 ∂ q˜ rkm ˜2 ∂ ∂ ∂ + r + ∂ ε˜ km ∂Dij ∂ q˜ km ∂Dij ∂Dij

D∇ ij −

˜ s∇ ∂ γ ≥0 ∂γijs ij (9.227b)

Using (9.212) and noting that Nijkm is the inverse of Mijkm , (9.227a) reduces to σ˜ ij =

˜1 ∂ ∂ ε˜ ij

(9.228)

˜ 1 (˜εij , q˜ r ). Also, (9.227b) Thus, the effective stress is derivable from potential ij can be rearranged to yield ˜ 1 r∇ ˜2 ˜ 2 s∇ ∂ ∂ ∂ − r q˜ km + Gij − D∇ γ ≥0 ij − ∂ q˜ km ∂Dij ∂γijs ij

© 2005 by Chapman & Hall/CRC Press

(9.229)

524

Continuum Mechanics and Plasticity

where Gij =

˜ 1 ∂ ε˜ km ∂ ε˜ km ∂ = −σ˜ km ∂ ε˜ km ∂Dij ∂Dij

(9.230)

In the derivation, (9.228) and (9.219) were used. Note that the ﬁrst term of (9.227b) and the second term in the bracket of the same inequality are combined to form the ﬁrst term of (9.229). From the assumption that damage does not directly inﬂuence the state of ﬁctitious plasticity, that is, damage affects the deformation only through Dij , the constraint (9.229) can be replaced by the following stronger conditions ˜1 ∂ − r q˜ r∇ ≥0 ∂ q˜ ij ij

˜2 ∂ Gij − ∂Dij

and

D∇ ij −

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.231)

The conditions apply, respectively, to the ﬁctitious plastic deformation process and the damage process. Furthermore, if the values of εij , Dij , qrij , and γijs ˜ 2 are also ﬁxed, since Gij is a function of are ﬁxed, then the values of Gij and ˜ 2 is a state function. For inequalstate variables as deﬁned by (9.230), and ity (9.231b) not to be violated for an arbitrary choice of D∇ ij , the following conditions must hold Gij =

˜2 ∂ ∂Dij

and

−

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.232)

For a more detailed investigation of a CDM model, the damage tensor Dij can be divided into two parts, that is, Dij = Drij + Dnij

(9.233)

The recoverable part Drij is due to area reduction associated with the growth of microdefects that can be recovered during unloading. The nonrecoverable part Dnij involves the reduction of area due to the extension of existing microcracks and/or the nucleation of microdefects. In summary, the constitutive equations for an isothermal damaged continuum are given by the following sets of equations and constraints σ˜ ij =

˜1 ∂ ∂ ε˜ ij

with −

˜ 1 r∇ ∂ q˜ ≥ 0 ∂ q˜ rij ij

(9.234)

Gij =

˜2 ∂ ∂Dij

with −

˜ 2 s∇ ∂ γ ≥0 ∂γijs ij

(9.235)

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

525

and Gij = −

˜ 1 ∂ ε˜ km ∂ ∂ ε˜ km ∂Dij

(9.236)

Equation (9.234) characterizes the deformation of the ﬁctitious undamaged continuum, and the inequality of (9.234) constrains the evolution of plastic internal variables. The set of equation and constraint (9.235) provides a relationship between the damage force Gij and the damage measure Dij . It also provides a constraint on the evolution of damage internal variables. Finally, the coupling between the deformation process and damage process is provided by (9.236). This is further explained in the subsequent paragraph. Consider a ﬁctitious, undamaged, element subjected to loading increment ˜ dPi . During loading, there are various forms of dissipation of energy associated with plasticity and damage processes. In particular, the rate of energy dissipation (caused by the damage force) due to a unit damage growth D∇ ij ∇ ˜ with respect to the ﬁctitious element is (∂ 2 /∂Dij )D . At the end of the loadij

ing period, it is required that the ﬁctitious element returns to its undamaged state before the next loading can be applied. The restoring energy associated with this transformation is given by −Gij D∇ ij , where −Gij is the restoring force. Because the damage needed to be restored at the end of a loading period is equal to the negative of the damage growth during loading, the force associated with the two processes must be equal in magnitude. Therefore, (9.236) can be viewed as a constraint that must be satisﬁed for the ﬁctitious deformation and damage process to occur simultaneously within the same continuum. In fact, this is a required constraint that arrives naturally from thermodynamic consideration. Equations and constraints in (9.234) to (9.236) provide a framework for theories of CDM. Explicit constitutive equations may be obtained if functions ˜ 1 and ˜ 2 are speciﬁed. Explicit evolution equations, which satisfy the for inequalities of (9.234) and (9.235), for internal variables qrij , and γijs should also be given. Different theories may be proposed based on this constitutive framework. One such theory has been formulated by Wu and Nanakorn [65] by use of the concept of endochronic plasticity. In that paper, the model has been applied to a one-dimensional case that describes uniaxial monotonic compression and tension of a concrete specimen. It successfully describes the strain-softening behavior after the peak load. In addition, the model has been applied to the description of deformation behavior for cyclically loaded concrete and mortar specimens. Satisfactory results have been obtained. It is remarked that the internal variables are not observable. Using the evolution equations for these variables, these variables do not necessarily appear in the ﬁnal form of the constitutive equations. Depending on the functional ˜ 1 and ˜ 2 and the explicit forms for the evolution equations for qr , forms for ij and γijs , a set of macroscopic parameters may be used for the model. These parameters may then be determined from experiments.

© 2005 by Chapman & Hall/CRC Press

526

Continuum Mechanics and Plasticity

9.5.7

A Brief Summary of Wu and Nanakorn’s Endochronic CDM

Several CDM models based on endochronic theory of plasticity have been proposed. The model of Valanis [66] is for brittle materials, while the models of Niu [67] and Chow and Chen [68] are for ductile materials. The model of Niu [67] is limited to isotropic damage due to the scalar representation of damage; the model of Chow and Chen [68] is an anisotropic damage model. Wu and Nanakorn’s model [65] is applicable to ductile materials with anisotropic damage. The equations of the Wu–Nanakorn model are summarized in this section for later references with permission from ASCE. This model is different from that of Chow and Chen [68], which uses neither the damage internal variables γijs nor the concept of damage restoring force Gij . Instead, Chow and Chen [68] uses Dij as an internal variable and express the damage evolution equations in terms of the potential of damage dissipation and elastic strain energy release rate Yij . In the Wu–Nanakorn model, the governing equations and constraints are given by (9.234) to (9.236). In this section, explicit forms of equations ˜ 1 (˜εij , q˜ r ) and are derived by assuming the following quadratic forms for ij ˜ 2 (Dij , γ s ): ij

1 ˜ 1 ε˜ ij , q˜ rij = Aijkm ε˜ ij − q˜ rij ε˜ km − q˜ rkm 2 r

1 s ˜ 2 Dij , γijs = Hijkm Dij − γijs Dkm − γkm 2 r

(9.237) (9.238)

where Aijkm and Hijkm are positive semi-deﬁnite fourth-rank isotropic tensors. The free energies in (9.237) and (9.238) are deﬁned on the ﬁctitious undamaged material, which is isotropic. Represent now any fourth-order isotropic tensor Wijkm by W2 Wijkm = W1 δij δkm + W2 δik δjm , with W0 = 3 W1 + (9.239) 3 where W1 and W2 are constants, and symmetry of Wijkm with respect to k and m is assumed. Also, the variables may be decomposed into the deviatoric and hydrostatic parts as σ˜ ij = σ˜ ij + 13 δij σ˜ kk ,

ε˜ ij = e˜ij + 13 δij ε˜ kk ,

q˜ rij = p˜ ijr + 13 δij q˜ rkk

(9.240)

and Gij = gij + 13 δij Gkk ,

Dij = dij + 13 δij Dkk ,

s γijs = rijs + 13 δij γkk

(9.241)

Using these notations, the explicit form of constitutive equations for damaged materials may be derived and are presented in the remaining part of this section.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

527

9.5.7.1 Equations of plastic deformation The deformation behavior is characterized by the effective stress-effective strain relationship given in (9.234). Using (9.237), this equation reduces to the following two equations by separating hydrostatic and deviatoric components: σ˜ kk =

Ar0 (˜εkk − q˜ rkk )

(9.242)

Ar2 (˜eij − p˜ ijr )

(9.243)

r

σ˜ ij =

r

where Ar0 and Ar2 are deﬁned by (9.239) with W replaced by A. Within a linear assumption, the evolution equations for the hydrostatic and deviatoric parts of q˜ rij are given in the following form Lr0

d˜qrkk d˜zH

∇ − σ˜ kk = 0

and

Lr2

d˜pijr d˜zD

∇ − σ˜ ij = 0

(9.244)

where ( )∇ indicates that the differentiation operator in bracket is corotational; Lr0 and Lr2 are constants; and d˜z deﬁnes the intrinsic time with respect to the ﬁctitious deformation. The intrinsic time is divided into the hydrostatic and deviatoric parts. An hydrostatic intrinsic time measure ζH is deﬁned to register the hydrostatic deformation. It is scaled by the intrinsic time scale zH so that it can properly describe strain hardening. They are related by $ $ $ dσ˜ kk $$ $ dζH = $d˜εkk − k1 3K $

with

0

dζH = h (ζH ) > 0 dzH

(9.245)

where 0 ≤ k1 ≤ 1 and K0 is the Bulk Modulus. The deviatoric intrinsic time ˜ ij which is given by ζD is deﬁned based on an effective strain-like tensor Q ˜ ij =∇ d˜eij − k2 dQ

∇

∇dσ ˜ ij

2µ0

(9.246)

where 0 ≤ k2 ≤ 1 and µ0 is the shear modulus. The operator ∇d denotes the corotational increment and is deﬁned on a second-order tensor aij with respect to the intrinsic time z as ∇

daij = t daij − Wik akj dz + aik Wkj dz

(9.247)

where t d denotes the increment based on material rate and Wij is the spin tensor. The deviatoric intrinsic time is deﬁned and scaled as follows: ˜ ij ∇ dQ ˜ ij dζD2 = ∇dQ

© 2005 by Chapman & Hall/CRC Press

with

dζD = f (ζD ) > 0 dzD

(9.248)

528

Continuum Mechanics and Plasticity

In (9.245) and (9.248), h(ζH ) and f (ζD ) are the strain-hardening functions corresponding to the hydrostatic and deviatoric deformation, respectively. 9.5.7.2 Equations of damage Equations (9.235) and (9.238) lead to the following relations for the hydrostatic and deviatoric parts of damage force Gij , respectively, Gkk =

s H0s Dkk − γkk ,

gij =

s

H2s dij − rijs

(9.249)

s

where H0s and H2s are constants. In the hydrostatic damage, microdefects expand and contract such that the overall symmetric properties of the material, that is, all planes of symmetry, are retained. In the deviatoric damage, the orientation of microcracks and microvoids changes, resulting in changes of overall symmetry properties and inducing the anisotropic behavior of the material. Using the inequality of (9.235), the linear evolution equations of γijs can be further separated into hydrostatic and deviatoric parts as J0s

s dγkk d dzH

∇

− Gkk = 0

and

J2s

drijs d dzD

∇ − gij = 0

(9.250)

d and dzd are the damage intrinsic time where J0s and J2s are constants; dzH D increment corresponding to the hydrostatic and deviatoric damage, respectively. The hydrostatic damage intrinsic time and its timescale are deﬁned, respectively, by

$ $ $ dGkk $$ d = $$dDkk − k3 dζH 3B $ 0

with

d dζH d dzH

d = hd ζH >0

(9.251)

where 0 ≤ k3 ≤ 1 and B0 is a material constant. Similarly, the deviatoric damage intrinsic time and its timescale are deﬁned by d 2 dζD = ∇dRij ∇dRij

with

= f d ζDd > 0

dζDd d dzD

(9.252)

where the damage-like tensor ∇dRij is deﬁned by ∇

dRij = ∇ddij − k4

∇dg

ij

2M0

(9.253)

with 0 ≤ k4 ≤ 1 and M0 is a material constant. The role played by material constants B0 and M0 in the Gij versus Dij relationship is similar to that played

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

529

by the bulk modulus K0 and shear modulus µ0 in the stress–strain relationd ) and f d (ζ d ) describe the material damage resisting ship. The functions hd (ζH D (hardening) behavior, which increases the damage threshold. These functions are similar to the hardening functions h(ζH ) and f (ζD ) of plastic deformation, but with a different physical meaning. The role played by (9.251) and (9.252) in damage is analogous to that played by (9.245) and (9.248) in the stress–strain space for the limit case of ki → 1 (i = 1, 2, 3, 4). The relations (9.251a) and (9.253) can be interpreted as the nonrecoverable hydrostatic and deviatoric parts of the damage tensor increment dDij , respectively. Note that ζ d is deﬁned in terms of the nonrecoverable damp age Dnij rather than the effective plastic strain ε˜ ij , as in the theories of Niu [67] and Chow and Chen [68]. This new damage intrinsic time enables the present theory to describe the behavior of damage in brittle materials, where damage occurs within the elastic range, as well as in ductile materials. 9.5.7.3

Coupling between deformation and damage

The coupling between deformation and damage processes is achieved through the damage force Gij given by (9.236). Using the quadratic form of ˜ 1 (˜εij , q˜ r ) given in (9.237), (9.236) reduces to ij

∂ ε˜ uv ∇ ) ∂Dij r dNpquv ∇ =− Aruvmn ε˜ mn − q˜ rmn εpq dDij r

Gij = −

Aruvmn (˜εmn − q˜ rmn )(

(9.254)

This equation relates the damage force Gij to the effective strain ε˜ ij and effective internal variables q˜ rij , both of which are responsible for the deformation process of the ﬁctitious continuum. On the other hand, the damage force is ˜ 2 (Dij , γ s ) by (9.235), which, by use of (9.238), related to the damage potential ij reduces to Gij =

˜2 ∂ s s Dkm − γkm = Hijkm ∂Dij s

(9.255)

This equation relates damage force Gij to the damage tensor Dij and internal variables γijs . The interpretations of (9.254) and (9.255) are as follows: consider a ﬁctitious, undamaged, material element subjected to a loading increment. During loading, different forms of energy associated with plasticity and damage process are dissipated. In particular, the rate of energy dissipation ∇ due to damage growth D∇ ij in the ﬁctitious element is (∂2 /∂Dij )Dij . At the end of the loading period, it is required that the ﬁctitious element returns to its undamaged state before the next loading can be applied. The restoring energy

© 2005 by Chapman & Hall/CRC Press

530

Continuum Mechanics and Plasticity

associated with this process is −Gij D∇ ij , where −Gij is the restoring force and the negative of the restoring force, Gij , is given by (9.254). Because the damage to be restored at the end of the loading period is equal to the negative of the damage growth during loading, the force associated with the two processes must be equal in magnitude. Therefore, (9.255) with Gij deﬁned by (9.254), can be viewed as a constraint that must be satisﬁed for the deformation and damage processes to occur simultaneously within the ﬁctitious continuum. In fact, this is a required constraint which arises naturally from the thermodynamic consideration. 9.5.8

Application

In this section, the model of the previous section is applied to investigate the problem of a cylindrical concrete specimen subjected to uniaxial compression in the x3 -direction. For such a problem, the state of stress and strain is given by 0 0 0 0 ε11 0 [σ ] = 0 0 0 [ε] = 0 ε22 0 (9.256) 0 0 σ33 0 0 ε33 where ε33 is prescribed for a strain control test. These are the principal stress and strain components and the directions of principal damage coincide with those of the principal stress and strain, if the specimen is initially isotropic and is subjected to proportional loading. In this case, the corotational rate reduces to the material rate. The increments of effective stress and effective strain are 0 0 0 0 0 d˜ε11 0 d˜ε22 0 [dσ˜ ] = 0 0 [d˜ε ] = 0 (9.257) 0 0 dσ˜ 33 0 0 d˜ε33 Their deviatoric parts are 0 0 −dσ˜ 33 1 −dσ˜ 33 0 [dσ˜ ] = 0 3 0 0 2 dσ˜ 33 0 (2 d˜ε11 − d˜ε22 −d˜ε33 ) 1 0 (−d˜ε11 + 2 d˜ε22 [d˜e] = −d˜ε33 ) 3 0 0

0

0 (−d˜ε11 − d˜ε22 +2 d˜ε33 )

(9.258)

The damage-effect tensor Mijkm is selected according to Betten’s deﬁnition of effective stress. Using (9.179) and (9.188), this tensor and its inverse are

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

531

expressed in the matrix form as

1 (1 − D1 )2 0 [M] = 0 [N] =

(1 − D1 )2

0

0

1 (1 − D2 )2

0

0

1 (1 − D3 )2

(9.259)

(1 − D2 )2

(1 − D3 )2

where D1 , D2 , and D3 are the principal damage in the x1 , x2 , and x3 directions, respectively. In this example, for the sake of simplicity, only one internal variable each for q˜ ij and γij is used. The use of only one internal variable was shown in previous applications of endochronic plasticity to be capable of capturing the main features of stress–strain responses in a plastically deformed continuum. The hydrostatic behavior of the ﬁctitious deformation is now considered. Combining (9.242), (9.244a) and (9.245a), the following equation is obtained dσ˜ kk dσ˜ kk ± k1 X = (1 ± X)d˜εkk A0 3K0

with X =

σ˜ kk L0 h(ζH )

(9.260)

where A0 and L0 are constants. The minus (−) and plus (+) signs, in (9.260), correspond to tension and compression, respectively. The material constant A0 may be identiﬁed with the bulk modulus 3K0 by considering the ﬁctitious undamaged material at its initial loading state, where σ˜ kk = q˜ kk = 0. Using the effective stress and effective strain of (9.257), (9.260) becomes dσ˜ 33 = 3K0 F(k1 , X)(d˜ε11 + d˜ε22 + d˜ε33 )

(9.261)

σ˜ 33 L0 h(ζH )

(9.262)

where F(k1 , X) =

1±X 1 ± k1 X

and

X=

The deviatoric response of the ﬁctitious undamaged material, from (9.243), (9.244b), and (9.258), is described by A2 σ˜ 33 dzD L2 A2 σ˜ 33 − dσ˜ 33 = A2 (−d˜ε11 + 2 d˜ε22 − d˜ε33 ) + dzD L2 A2 σ˜ 33 2 dσ˜ 33 = A2 (−d˜ε11 − d˜ε22 + 2 d˜ε33 ) − dzD L2 − dσ˜ 33 = A2 (2 d˜ε11 − d˜ε22 − d˜ε33 ) +

© 2005 by Chapman & Hall/CRC Press

(9.263a) (9.263b) (9.263c)

532

Continuum Mechanics and Plasticity

Equation (9.261) and the two independent equations of (9.263) can be put in the matrix form as 1 −3K0 F(k1 , X) −3K0 F(k1 , X) dσ˜ 33 0 1 d˜ε11 + 1 A2 σ˜ 33 dzD 2A2 −A2 L2 1 1 −A2 2A2 d˜ε22 3K0 F(k1 , X) d˜ε33 A2 = (9.264) A2 where dzD is related to the deviatoric components of the incremental effective strain d˜εij and its relationship is now discussed. The following expression may be found from (9.246) ˜ ij = ϕij + ψij dzD dQ

(9.265)

where ϕij = (1 − k2 )d˜eij

and

ψij =

k2 σ˜ ij

(9.266)

L2

By use of (9.248) and (9.265), the relation for dzD is obtained as 2 ϕij ϕij + 2ϕij ψij dzD + [ψij ψij − f (ζD )2 ]dzD =0

(9.267)

The equation of hydrostatic damage is found from (9.249a), (9.250a), and (9.251a) as dGkk dGkk ± k3 Y = (1 ± Y) dDkk H0 3B0

with Y =

Gkk d) J0 hd (ζH

(9.268)

where H0 , B0 , and J0 are material constants. Considering the initial loading state, where Gkk = γkk = 0, it may be shown that H0 is the initial slope of the Gkk versus Dkk curve and that H0 = 3B0 . The minus (−) and plus (+) signs, in (9.268), correspond to tension and compression, respectively. Equation (9.268a) further reduces to dGkk = H0 F(k3 , Y) dDkk

with F(k3 , Y) =

1±Y 1 ± k3 Y

(9.269)

The equation for deviatoric damage response may be obtained from (9.249b) and (9.250b) as gij d dgij = H2 ddij + dzD J2

© 2005 by Chapman & Hall/CRC Press

(9.270)

Topics in Endochronic Plasticity

533

where H2 and J2 are constants and H2 may be identiﬁed with the initial slope of the deviatoric Gij versus Dij curve. Furthermore, H2 = 2M0 . The damd is related to the deviatoric components of age intrinsic time increment dzD the damage force increment dgij and its relationship is now discussed. The following expression may be found from (9.253) and (9.270) d dRij = ϕijd + ψijd dzD

(9.271)

where ϕijd = (1 − k4 )

dgij H2

and

ψijd =

gij J2

(9.272)

d is obtained as By use of (9.252a) and (9.271), the relation for dzD

d 2 d + ψijd ψijd − f d (ζDd )2 (dzD ) =0 ϕijd ϕijd + 2ϕijd ψijd dzD

(9.273)

Using (9.236) and (9.257), the damage force Gij reduces to Gij = −σ˜ km

∂ ε˜ km ∂ ε˜ 33 = −σ˜ 33 ∂Dij ∂Dij

(9.274)

Since ε˜ 33 = (1 − D3 )2 ε33 , ε˜ 33 does not depend on D1 and D2 . Consequently, the only nonzero component of tensor Gij is G33 =

2σ˜ 33 ε˜ 33 1 − D3

(9.275)

and its increment is found to be dG33 =

2σ˜ 33 2˜ε33 2σ˜ 33 ε˜ 33 d˜ε33 + dσ˜ 33 + dD3 1 − D3 1 − D3 (1 − D3 )2

(9.276)

Thus, the deviatoric part of the increment of the damage force is

−dG33 1 [dgij ] = 0 3 0

0 −dG33 0

0 0 2dG33

(9.277)

Furthermore, 0 0 2 dD1 − dD2 − dD3 1 0 0 −dD1 + 2 dD2 − dD3 [ddij ] = 3 0 0 −dD1 − dD2 + 2 dD3 (9.278)

© 2005 by Chapman & Hall/CRC Press

534

Continuum Mechanics and Plasticity

Equations (9.277) and (9.278) are substituted into (105) and the two independent equations of (9.269) to obtain the following matrix equation for the damage process:

H0 F(k3 , Y) H0 F(k3 , Y) H0 F(k3 , Y) dD1 2H2 −H2 −H2 dD2 −H2 2H2 −H2 dD3 1 0 H2 G33 d = −1 dG33 − 1 dzD J2 −1 1

(9.279)

The equations derived in this section are now applied to the problem of uniaxial compression of cylindrical concrete specimen (fc = 73.8 MPa and E=27.6 GPa). To determine the material parameters for the model, the analytical stress–strain curves obtained by Fonseka and Krajcinovic [69] is used. In this case, the directions of the principal damage coincide with those of the principal stress. The procedure of calculation is now described. An increment d˜ε33 is ﬁrst speciﬁed. An initial value for dzD is assumed and (9.264) solved for dσ˜ 33 , d˜ε11 , and d˜ε22 . These values are then used in (9.267) to solve for dzD . An iteration procedure is applied to determine dG33 . (9.273) d . Thus, dD , dD , and dD are found is subsequently used to determine dzD 1 2 3 from (9.279). An iteration procedure is also applied on dD3 to determine its value, which corresponds to the speciﬁed d˜ε33 . Knowing d˜ε33 and dD3 , dε33 can be calculated from the incremental form of ε33 =

ε˜ 33 (1 − D3 )2

(9.280)

This procedure continues for another speciﬁed d˜ε33 . Using a trial-and-error (curve-ﬁtting) procedure, the following material parameters for the deformation equations have been determined: Poisson’s ratio = 0.2, effective hydrostatic yield stress L0 = 4.55 MPa, effective deviatoric yield stress L2 = 18.61 MPa, strain-hardening parameters µH = µd = 0, and k1 = k2 = 0.95. The material parameters for the damage equations have been found to be: hydrostatic damage modulus H0 = 0.78 MPa, deviatoric damage modulus H2 = 1.91 MPa, hydrostatic damage threshold J0 = 0.61 MPa, deviatoric damage threshold J2 = 1.93 MPa, damage resisting (hardening) parameters µdH = µdD = 0, and k3 = k4 = 0.95. The computed stress–strain curves are plotted in Figure 9.22. There are two curves in this ﬁgure. One curve is for the axial strain and the other for the lateral strain. The volumetric strain versus compressive stress is plotted in Figure 9.23. The curve shows a change of sign of the volumetric strain as the axial strain increases. The volumetric strain is initially negative and it changes to positive when the axial strain becomes large in magnitude. This phenomenon is typical in concrete and rocks, and it is due to the increase

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

535 Compressive stress (MPa)

60 40 Endochronic 20 Fonseka and Krajcinovic (1981) Strain (%) –0.2

–0.4

0.2

Axial Strain

Lateral Strain

FIGURE 9.22 Stress versus axial and lateral strains in uniaxial compression of concrete (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

Compressive Stress (MPa) Endochronic Fonseka and Krajcinovic (1981)

60 40 20

–0.1

–0.05

0.05

0.1

Volumetric Strain (%) FIGURE 9.23 Stress versus volumetric strain in uniaxial compression of concrete (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

in the lateral-to-axial strain ratio (−ε11 /ε33 ) as the axial strain increases. It is seen in Figure 9.24 that this ratio changes from 0.2 to approximately 0.6 as the axial compressive strain increases from 0 to 0.005. The results of this model presented in Figure 9.22 and Figure 9.23 show good agreement with the computed value obtained by Fonseka and Krajcinovic [69].

9.5.9

Concluding Remarks

The concepts of CDM have been discussed and a constitutive framework of CDM has been developed based on the internal variables approach. The framework involves transforming the actual damaged continuum into an equivalent ﬁctitious undamaged continuum. The effects of damage are

© 2005 by Chapman & Hall/CRC Press

Continuum Mechanics and Plasticity

The –11/33 Ratio

536

0.5 0.4 0.3 0.2 0.1

0.2

0.3

0.4

0.5

Axial strain 33 (%) FIGURE 9.24 Lateral to axial strain ratio versus axial compressive strain (From Wu, H.C. and Nanakorn, C.K., Int. J. Solids Struct., 36, 5057, 1999. With permission from Elsevier).

accounted for by replacing the actual stress σij (gross stress) on the damaged continuum with the symmetric effective stress σ˜ ij . Adistinction has been made between the state of damage and the damage measure Dij and the concept of “damage force” has been introduced. Within the proposed constitutive framework, the endochronic concept has been used to derive explicit constitutive equations. Two intrinsic times are used in the formulation. The ﬁrst intrinsic time ζ is used to describe the plastic deformation history of the ﬁctitious undamaged continuum and the second intrinsic time ζ d is used to depict the damage history. The model is applicable to both brittle and ductile materials with damage. The following conclusions may be drawn from this study: 1. The damage tensor Dij may be deﬁned based on a second-order continuity tensor ψij . 2. The damage-effect tensor Mijkm deﬁned by Betten [58] gives rise to an effective stress that has a simple physical interpretation, while other deﬁnitions of Mijkm do not have the same signiﬁcance. 3. The transformation equation for effective strain, (9.214), may be derived based on the free energy equivalence postulate. 4. In addition to damage tensor Dij , which is a measurable quantity, a set of damage internal variables γijs , which are not measurable, is used in the formulation. 5. The constitutive equations for an isothermal damaged continuum include two sets of equations and constraints. The ﬁrst set characterizes the deformation of the ﬁctitious undamaged continuum and constrains the evolution of plastic internal variables qrij . The second set provides a relationship between the damage force Gij and the damage measure Dij . It also provides a constraint on the evolution of damage internal variables γijs . In addition, (9.236) must be used to complete the constitutive equations. This equation is a constraint that

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

537

must be satisﬁed for the ﬁctitious deformation and damage process to occur simultaneously within the same continuum. 6. The theory does not use the concepts of yield surface or damage surface as its prime requisite although both surfaces may be deﬁned when necessary by setting all ki = 1. Therefore, the constitutive equations of this theory are continuous without discontinuities, which is advantageous in the numerical calculation. 7. The proposed model has been shown to describe the threedimensional state of deformation of a cylindrical concrete specimen subjected to uniaxial compression. The focal point of the work of Wu and Nanakorn [54] is to formulate a constitutive framework that is self-consistent. Some well-known concepts have been discussed and it has been pointed out that some concepts are not compatible with others. Only concepts that are compatible to each other are used in the derivation. New concept such as the distinction between the state of damage and damage measure and the concept to restore the ﬁctitious continuum to its undamaged state after each step of deformation and damage have been introduced. Finally, we mention that we use the corotational rate to account for rotation of principal damage directions during deformation.

References 1. Wu, H.C. and Yeh, W.C., Some considerations in the endochronic description of anisotropic hardening, Acta Mech., 69, 59, 1987. 2. Ohashi, Y., Tokuda, M., Mitake, T., Kurita, Y., and Suzuki, T., Stress–strain relation of integral type for deformation of brass along strain trajectories consisting of three normal straight branches, Arch. Mech., 32, 125, 1980. 3. Ohashi, Y., Tokuda, M., Suzuki, T., and Kurita, Y., Stress–strain relation of brass for the plastic deformation along bi-linear strain trajectories with various corner angles, Bull. Japan. Soc. Mech. Eng., 24, 1909, 1981. 4. Wu, H.C., Hong, H.K., and Lu, J.K., An endochronic theory accounted for deformation induced anisotropy, Int. J. Plasticity, 11, 145, 1995. 5. Wu, H.C., Lu, J.K., and Pan, W.F., Endochronic equations for ﬁnite plastic deformation and application to metal tube under torsion, Int. J. Solids Struct., 32, 1079, 1995. 6. Phillips, A. and Tang, J.L., The effect of loading path on the yield surface at elevated temperatures, Int. J. Solids Struct., 8, 463, 1972. 7. Wu, H.C. and Yeh, W.C., On the experimental determination of yield surfaces and some results of annealed 304 stainless steel, Int. J. Plasticity, 7, 803, 1991. 8. Wu, H.C. and Lu, J.K., Further development and application of an endochronic theory accounted for deformation induced anisotropy, Acta Mech., 109, 11, 1995.

© 2005 by Chapman & Hall/CRC Press

538

Continuum Mechanics and Plasticity

9. Wu, H.C. and Hong, H.K., Endochronic description of plastic anisotropy in sheet metal, Int. J. Solids Struct., 36, 2735, 1999. 10. Hill, R., A theory of yielding and plastic ﬂow of anisotropic materials, Proc. Roy. Soc., London, A, 193, 281, 1948. 11. Valanis, K.C., A theory of viscoplasticity without a yield surface, Arch. Mech. 23, 517, 1971. 12. Valanis, K.C., Proper tensorial formulation of the internal variable theory, The endochronic time spectrum, Arch. Mech., 29, 173, 1977. 13. Valanis, K.C., Back stress and Jaumann rates in ﬁnite plasticity, Int. J. Plasticity, 6, 353, 1990. 14. Dafalias, Y.F., Plastic spin: necessity or redundancy?, Int. J. Plasticity, 14, 909, 1998. 15. Im, S. and Atluri, S.N., A study of two ﬁnite strain plasticity models: an internal time theory using Mandel’s director concept, and a general isotropic/kinematic-hardening theory, Int. J. Plasticity, 3, 163, 1987. 16. Goddard, J.D. and Miller, C., An inverse for the Jaumann derivative and some applications to the rheology of viscoelastic ﬂuids, Rheol. Acta, 5, 177, 1966. 17. Dafalias, Y.F., Corotational integral in constitutive formulations, J. Eng. Mech., 113, 1967, 1987. 18. Swift, H.W., Length change in metal under torsional overstrain, Engineering, 163, 253, 1947. 19. Hart, E.W. and Chang, Y.W., Material rotation effects in tension–torsion test: experimental result, in Plasticity Today, Sawczuck, A. and Bianchi, G.E., Eds., Elsevier Appl. Sci., U.K., 1985, 235. 20. White, C.S., Bronkhorst, C.A., and Anand, L., An improved isotropickinematic hardening model for moderate deformation metal plasticity, Mech. Mater., 10, 127, 1990. 21. Wu, H.C. and Xu, Z.Y., An extensometer investigation of the axial effect during torsion. Proc. Int. Conf. on Constitutive Laws for Eng. Material, Fan, J. and Murakami, S., Eds., Chongqing, China, 1989, 232. 22. Bailey, J.A., Haas, S.L., and Nawab, K.C., Anisotropy in Plastic Torsion, J. Basic Eng., 94, 231, 1972. 23. Wu, H.C., Xu, Z., and Wang, P.T., Torsion test of aluminum in the large strain range, Int. J. Plasticity, 13, 873, 1998. 24. Canova, G.R., Kocks, U.F., and Jonas, J.J., Theory of torsion texture development, Acta Metall., 32, 211, 1984. 25. Taylor, G.I. and Quinney, H., The plastic distortion of metal, Phil. Trans. Roy. Soc., A, 230, 323, 1932. 26. Lowe, T.C. and Lipkin, J., Analysis of axial deformation response during reverse shear, Sand90-8417, Sandia National Lab., 1990. 27. Qian, Z. and Wu, H.C., A 2-D texture study based on a double-slip model of polycrystal plasticity with analysis of thin-walled tube under torsion, Int. J. Solids Struct., 33, 4167, 1996. 28. Wu, H.C. and Aboutorabi, M.R., Endochronic modeling of coupled volumetric–deviatoric behavior of porous and granular materials, Int. J. Plasticity, 4, 163, 1988. 29. Wu, H.C., An endochronic theory for porous and granular materials, in Modern Approaches to Plasticity, Kolymbas, D., Ed., Elsevier, Amsterdam, 1993, 347.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

539

30. Johnson, J.N. and Green, S.J., Mechanical response of porous media subject to static load, in Effects of Voids on Material Deformation, Cowin, S.C. and Carroll, M.M., Eds., AMD-16, ASME, New York, 1976, 93. 31. Scavuzzo, R., Stankowski, T., Gerstle, K.H., and Ko, H.Y., Stress–strain curves for concrete under multiaxial load histories, Report, Department of Civil, Environmental and Architectural Engineering, University of Colorado, Boulder, CO, 1983. 32. Wu, H.C., Wang, Z.K., and Aboutorabi, M.R., Endochronic modeling of sand in true triaxial test, J. Eng. Mech., ASCE, 111, 1257, 1985. 33. Bazant, Z.P. and Krizek, R.J., Endochronic constitutive law for liquefaction of sand, J. Eng. Mech. Div., ASCE, 102, 225, 1976. 34. Valanis, K.C. and Read, H.E., A new endochronic plasticity model for soils, in Soil Mechanics-Transient and Cyclic Loads, Pande, G.N. and Zienkiewicz, O.C., Eds., John Wiley, New York, 1982. 35. Valanis, K.C. and Peters, J.F., Conﬁgurational plasticity in granular media, in Modern Approaches to Plasticity, Kolymbas, D., Ed., Elsevier, Amsterdam, 1993, 1. 36. Wu, H.C., Wang, T.P., Endochronic description of sand response to static loading, J. Eng. Mech., ASCE, 109, 970, 1983. 37. Lade, P.V., Elasto-plastic stress–strain theory for cohesiveless soil with curved yield surfaces, Int. J. Solids Struct., 13, 1019, 1977. 38. Cuellar, V., Bazant, Z.P., Krizek, R.J., and Silver, M.L., Densiﬁcation and hysteresis of sand under cyclic shear, J. Geotechn. Eng. Division, ASCE, 103, 399, 1977. 39. Lee, K.L. and Seed, H.B., Drained strength characteristics of sands, J. Soil Mech. Found. Div., ASCE, 93, 117, 1967. 40. Wu, H.C. and Sheu, J.C., Endochronic modeling for shear hysteresis of sand, J. Geotechn. Eng., ASCE, 109, 1539, 1983. 41. Silver, M.L. and Seed, H.B., Deformation characteristic of sand under cyclic loading, J. Soil Mech. Found. Div., ASCE, 97, 1081, 1971. 42. Wu, H.C. and Aboutorabi, M.R., Endochronic model of sand with circular stress path, J. Geotechn. Eng., ASCE, 114, 93, 1988. 43. Aboutorabi, M.R., Wu, H.C., Wang, T.P., and Gao, Q.Y., Stress–strain behavior of porous aluminum, in Proc. 2nd International Conf. on Constitutive Laws for Engineering Materials: Theory and Application, Desai, C.S., Krempl, E., Kiousis, P.D., and Kundu, T., Eds., Elsevier, New York, 1987, 477. 44. Wang, P.T. and Wu, H.C., An endochronic model for compaction of porous metals, Prog. Powder Metall., 41, 161, 1986. 45. Schock, R.N., Abey, A.E., and Duba A., Quasi-static deformation of porous beryllium and aluminum, J. Appl. Phys., 47, 53, 1976. 46. Wu, H.C., Wang, P.T., Pan, W.F., and Xu, Z.Y., Cyclic stress–strain response of porous aluminum, Int. J. Plasticity, 6, 207, 1990. 47. Kachanov, L.M., On the time to failure during creep, Izv. AN. SSSR., OTN.337,1958. 48. Lemaitre, J. and Chaboche, J.L., Aspects phénoménologique ge la rupture par endommagement, J. Méc. Appl., 2, 167, 1978. 49. Sidoroff, F., Description of anisotropic damage application to elasticity, in Physical Non-Linearities in Structure Analysis-IUTAM, Hult, J. and Lemaitre, J., Eds., Springer-Verlag, New York, 1981, 237.

© 2005 by Chapman & Hall/CRC Press

540

Continuum Mechanics and Plasticity

50. Lemaitre, J. and Chaboche, J.L., Mécanique des Matériaux Solides, Paris: Dunod; English Edition, Cambridge University Press, 1985. 51. Chow, C.L. and Lu, T.J., A comparative study of continuum damage models for crack propagation under gross yielding, Int. J. Fract., 53, 43, 1992. 52. Chaboche, J.L., Sur l’utilisation des variables d’état interne pour la description du comportement viscoplastique et de la rupture par endommagement, Symposium Franco-Polonais de Rhéologie et Mécanique, Cracovie, 1977. 53. Lemaitre, J., A continuum damage mechanics model for ductile fracture, J. Eng. Mater. Technol., 107, 83, 1985. 54. Wu, H.C. and Nanakorn, C.K., A constitutive framework of plastically deformed damaged continuum and a formulation using the endochronic concept, Int. J. Solids Struct., 36, 5057, 1999. 55. Murakami, S. and Ohno, N., A continuum theory of creep and creep damage, in Creep Structures, Ponter A.R.S. and Hayhust, D.R., Eds., Springer, Berlin, 1981, 922. 56. Betten, J., Damage tensors in continuum mechanics, J. Mecanique theorique et appliqué, 2 , 13, 1983. 57. Rabotnov, Y.N., Creep Problems in Structural Members, North-Holland Series in Applied Math. and Mech., Vol. 7, Chap. 6, North-Holland, Amsterdam,1969. 58. Cordebois, J.P. and Sidoroff, F., Damage induced elastic anisotropy, Comportement mecanique des solides anisotropes, EUROMECH, 115, Proc. Coll., Int. du C.N.R.S., Boehler J.P. Ed., Villard-de-Lens, France, 1979, 761. 59. Chow, C.L. and Wang, J., An anisotropic theory of elasticity for continuum damage mechanics. Int. J. Fract., 33, 3, 1987. 60. Stumvoll, M. and Swobada, G., Deformation behavior of ductile solids containing anisotropic damage, J. Eng. Mech., 119, 1331, 1993. 61. Rabotnov, Y.N., Creep rupture, in Proceedings, Applied Mechanics Conference, Hetenyi, M. and Vincenti, H., Eds., Standford University, 1968, 342. 62. Chow, C.L. and Lu, T.J., On evolution laws of anisotropic damage, Eng. Fract. Mech., 34, 679, 1989. 63. Valanis, K.C., Irreversible Thermodynamics of Continuous Media, Springer-Verlag, Udine, 1971. 64. Krajcinovic, D., Continuous damage mechanics revisited: basic concepts and deﬁnition, ASME, J. Appl. Mech., 52, 829, 1985. 65. Wu, H.C. and Nanakorn, C.K., An endochronic theory of continuum damage mechanics, ASCE, J. Eng. Mech., 124, 200, 1998. 66. Valanis, K.C., A theory of damage in brittle materials, Eng. Fract. Mech., 36, 403, 1990. 67. Niu, X., Endochronic plastic constitutive equations coupled with isotropic damage and damage evolution models, Eur. J. Mech., A/Solids, 8, 293, 1989. 68. Chow, C.L. and Chen, X.F., An anisotropic model of damage mechanics based on endochronic theory of plasticity, Int. J. Fract., 55, 115, 1992. 69. Fonseka, G.U. and Krajcinovic, D., The continuous damage theory of brittle materials, part 2: uniaxial and plane response modes. J. Appl. Mech., 48, 816, 1981.

© 2005 by Chapman & Hall/CRC Press

Topics in Endochronic Plasticity

541

Problems (1) Start from (9.10) and derive (9.11). (2) Derive (9.13). (3) Show that if the intrinsic time is deﬁned by dζ 2 = dεp · K · dεp + tr(L · dεp ) dζ , then the corresponding yield function is (σ − α) · K · (σ − α) + σy f (z)tr[L · (σ − α)] = (σy f (z))2 .

(4) In (9.37), the evolution equations of internal variables qrx and qry are dqrx + Pr qrx + U r qry = Pr εx + U r εy dz dqry + Qr qry + V r qrx = Qr εy + V r εx dz where Pr , Qr , U r , and V r are not functions of qrx and qry . These two equations are coupled in qrx and qry . Decouple the equations. (5) Derive (9.45). (6) For the PG materials discussed in Section 9.4.1, derive the governing equations given by (9.127) to (9.130). (7) In the application to porous aluminum discussed in Section 9.4.4, derive (9.161) and (9.162) for the deviatoric stress–strain behavior.

© 2005 by Chapman & Hall/CRC Press

10 Anisotropic Plasticity for Sheet Metals

10.1

Introduction

Sheet metal is a special product form of a material that is produced by the rolling process. The process of rolling is illustrated by considering a strip of metal passing between a pair of rolls with their axes parallel to each other. The sheet metal enters the rolls, and the marginal speed of the rolls on the entry side is higher than the entry speed of the sheet. The friction forces created between the rolls and the metal strip tend to pull the strip into the gap between the rolls, where plastic deformation takes place. On exiting the rolls, the friction forces change direction and the sheet acquires a reduced thickness, while the speed of the sheet is greater than the speed of the rolls. The thickness of a metal sheet can be reduced further by additional rolling, generating various degrees of anisotropy. The anisotropy in the sheet metal is two-fold: the anisotropy in the yield stress and the anisotropy in the plastic ﬂow. The anisotropy is usually speciﬁed with respect to the rolling direction (RD) of the sheet (Figure 10.1); TD denotes the transverse direction and ND, the normal direction, which is not shown in the ﬁgure. Tension specimens cut at various angles θ measured counterclockwise from the rolling direction can exhibit different yield stresses and different characteristics of plastic deformation. Generally, both the yield stress and the plastic deformation are functions of the orientation angle θ . However, it is possible that a material does not show noticeable anisotropy in the yield stress but shows signiﬁcant anisotropy in the plastic deformation. The anisotropy of plastic ﬂow is usually measured by the plastic strain-ratio R, which is deﬁned by many recent researchers as p

R= p

dεw p

dεt

(10.1) p

where dεw is the plastic strain increment in the width direction, and dεt that in the thickness direction of a tension specimen. The value of R can vary from one sheet material to the other. It can be greater than one or less than one, and R = 1 implies material isotropy. The R-ratio is an important parameter 543

© 2005 by Chapman & Hall/CRC Press

544

Continuum Mechanics and Plasticity TD

RD

FIGURE 10.1 Tension specimen cut at angle θ .

of a sheet material. A large R means a small change in the thickness during longitudinal tension, while a small R corresponds to a large change in the thickness during longitudinal stretching. Therefore, a small R would lead to easy thinning and early failure of the sheet. This deﬁnition of R-ratio is not universal, however. Recent researchers prefer the deﬁnition of (10.1) because of its apparent tie to the ﬂow rule of plasticity. On the other hand, the ASTM Standards [1] deﬁne the R-ratio as R=

εw εt

where εw = ln

wf w0

and

εt = ln

tf t0

(10.2)

The subscripts ( )0 and ( )f denote the initial and ﬁnal lengths, respectively; w stands for width and t, the thickness. Thus, the R-ratio is the ratio between the true width strain and the true thickness strain. Due to the thinness of sheets, the thickness strain is difﬁcult to measure accurately. A practical method is to measure the longitudinal and width strains and make the assumption of volume constancy. Therefore, (10.2) reduces to R=

ln(w0 /wf ) ln(lf wf /l0 w0 )

(10.3)

where l is the longitudinal measurement. Many researchers believe that the R-ratio does not vary appreciably with strain and make the assumption of constancy in their theoretical analyses. Detailed information concerning the strain level at which the measurements of R were taken is generally not reported in the literature. Some measurements were taken after the specimens had undergone large deformation. Some were taken midway between the ﬁrst occurrence of nonuniform strain and the ﬁnal fracture. Tracking of the R-ratio during experiments has indicated, however, that the R-ratio may vary greatly with the increasing plastic strain [2]. Mellor [2] and Lin and Ding [3] noted further that, due to the inaccuracy of the experimental data, the R-ratio could not be assessed closer to the initial yield region of the material. The variation of R-ratio with increasing plastic strain is discussed later in this chapter.

© 2005 by Chapman & Hall/CRC Press

Anisotropic Plasticity for Sheet Metals

10.2

545

Standard Tests for Sheet Metal

10.2.1

The Uniaxial Tension Test

Tensile specimens are cut at predetermined angles θ (usually every 15◦ ) to the rolling direction. Uniaxial tension tests are conducted on these specimens and yield stress σθ determined as a function of θ. The stress state is given by σx = σθ cos2 θ ,

σy = σθ sin2 θ,

and σxy = σθ sin θ cos θ

(10.4)

After the test, strains in both the axial and width directions of the specimens are measured, and the thickness strain determined by the assumption of volume constancy.

10.2.2

Equibiaxial Tension Test

This experiment is performed to determine the equibiaxial yield stress σB . It can be accomplished by a self-designed loading frame attached to a universal test machine or a servo-hydraulic test system. When the sheet is thin and the static loading is of concern, the experiment could also be carried out by use of a self-designed dead-weight loading system. For a more versatile testing, two servo-controlled actuators may be placed 90◦ from each other to form the loading system.

10.2.3

Hydraulic Bulge Test

This test could also be used to determine the equibiaxial yield stress σB . In the bulge test, a thin disc of sheet metal is clamped around its periphery and then subjected to an increasing ﬂuid pressure applied to one side. The region in the vicinity of the dome becomes nearly spherical in shape as the sheet bulges. The tensile stresses in the plane of the sheet are the same by symmetry. An advantage of the bulge test is that it can be carried out to strains far greater than the instability strain in tension and is not complicated by friction as is the compression test. However, the test results are not direct. A boundary value problem has to be solved in which a constitutive equation is needed.

10.2.4

Through-Thickness Compression Test

Cylindrical specimens are prepared from discs of the sheet material glued together with an epoxy adhesive. The specimens were tested in compression using Teﬂon sheet and graphite grease for lubrication between the spec